Please copy and paste this embed script to where you want to embed

Time-Dependent Behaviour of Concrete Structures

Serviceability failures of concrete structures involving excessive cracking or deﬂection are relatively common, even in structures that comply with code requirements. This is often as a result of a failure to adequately account for the time-dependent deformations of concrete in the design of the structure. Design for serviceability is complicated by the non-linear and inelastic behaviour of concrete at service loads. The serviceability provisions embodied in codes of practice are relatively crude and, in some situations, may be unreliable and often do not adequately model the in-service behaviour of structures. In particular, they fail to realistically account for the effects of creep and shrinkage of the concrete. Providing detailed information, this book assists engineers to rationally predict the time-varying deformation of concrete structures under typical in-service conditions. It gives analytical methods to help anticipate time-dependent cracking, the gradual change in tension stiffening with time, creep-induced deformations and the load independent strains caused by shrinkage and temperature changes. Calculation procedures are illustrated with many worked examples. A vital guide for practising engineers and advanced students of structural engineering on the design of concrete structures for serviceability, providing a penetrating insight into the time-dependent behaviour of reinforced and prestressed concrete structures. Raymond Ian Gilbert is Professor of Civil Engineering at the University of New South Wales and currently holds an Australian Research Council Australian Professorial Fellowships. He has over 35 years experience in structural design and is a specialist in the analysis and design of reinforced and prestressed concrete structures. Gianluca Ranzi is a Senior Lecturer of Structural Engineering at the University of Sydney, specialising in the analysis and design of concrete and composite steel-concrete structures.

Time-Dependent Behaviour of Concrete Structures

Raymond Ian Gilbert and Gianluca Ranzi

First published 2011 by Spon Press 2 Park Square, Milton Park, Abingdon, Oxon OX14 4RN Simultaneously published in the USA and Canada by Spon Press 270 Madison Avenue, New York, NY 10016 USA

This edition published in the Taylor & Francis e-Library, 2010. To purchase your own copy of this or any of Taylor & Francis or Routledge’s collection of thousands of eBooks please go to www.eBookstore.tandf.co.uk. Spon Press is an imprint of the Taylor & Francis Group, an informa business © 2011 Raymond Ian Gilbert and Gianluca Ranzi All rights reserved. No part of this book may be reprinted or reproduced or utilised in any form or by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying and recording, or in any information storage or retrieval system, without permission in writing from the publishers. This publication presents material of a broad scope and applicability. Despite stringent efforts by all concerned in the publishing process, some typographical or editorial errors may occur, and readers are encouraged to bring these to our attention where they represent errors of substance. The publisher and author disclaim any liability, in whole or in part, arising from information contained in this publication. The reader is urged to consult with an appropriate licensed professional prior to taking any action or making any interpretation that is within the realm of a licensed professional practice. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library Library of Congress Cataloging-in-Publication Data Gilbert, R. I., 1950– Time-dependent behaviour of concrete structures / Raymond Ian Gilbert and Gianluca Ranzi. p. cm. Includes bibliographical references and index. 1. Concrete–Deterioration. 2. Service life (Engineering) 3. Concrete structures. I. Ranzi, Gianluca, 1972– II. Title. TA440.G449 2010 2010007786 624.1 834–dc22

ISBN 0-203-87939-2 Master e-book ISBN ISBN13: 978-0-415-49384-0 (hbk) ISBN13: 978-0-203-87939-9 (ebk)

Contents

Preface Acknowledgements Notation and sign convention

xi xiii xiv

1 Time-dependent deformation

1

1.1

1.2

1.3

1.4 1.5

Background 1 1.1.1 Concrete strain components 2 1.1.2 Typical concrete strain magnitudes 4 Creep of concrete 5 1.2.1 Creep mechanisms and inﬂuencing factors 5 1.2.2 Creep components 7 1.2.3 Effects of ageing 8 1.2.4 The creep coefﬁcient, ϕ (t, τ ), and the creep function, J (t, τ ) 8 1.2.5 The principle of superposition 9 1.2.6 Tensile creep 14 1.2.7 The effects of creep on structural behaviour 14 Shrinkage of concrete 17 1.3.1 Types of shrinkage 17 1.3.2 Factors affecting shrinkage 18 1.3.3 The effects of shrinkage on structural behaviour 18 Time analysis – the basic problem 22 References 22

2 Material properties 2.1

Concrete 24 2.1.1 Introductory remarks 24 2.1.2 Compressive and tensile strength 24 2.1.3 Elastic modulus 25 2.1.4 Creep coefﬁcient 26 2.1.5 Shrinkage strain 29

24

vi Contents 2.2

Steel reinforcement 31 2.2.1 General 31 2.2.2 Conventional, non-prestressed reinforcement 32 2.2.3 Prestressing steel 33 2.3 References 36

3 Design for serviceability – deﬂection and crack control 3.1 3.2 3.3 3.4

Introduction 37 Design objectives and criteria 38 Design actions 39 Design criteria for serviceability 41 3.4.1 Deﬂection limits 41 3.4.2 Crack width limits 44 3.5 Maximum span-to-depth ratio – minimum thickness 44 Example 3.1 48 3.6 Deﬂection control by simpliﬁed calculation 49 3.6.1 Calculation of deformation 49 3.6.2 Load versus deﬂection response of a reinforced concrete member 52 3.6.3 Modular ratio theory 54 3.6.4 AS 3600-2009 and ACI 318-08 57 3.6.4.1 3.6.4.2

3.6.5

Instantaneous deﬂection 57 Time-dependent deﬂection 58

Example 3.2 59 Eurocode 2 64 3.6.5.1 3.6.5.2

Instantaneous curvature 64 Time-dependent curvature 65

Example 3.3 65 3.6.6 Recommended simpliﬁed approach 69 3.6.6.1 3.6.6.2 3.6.6.3

3.7

Instantaneous deﬂection 69 Time-dependent creep-induced curvature 70 Time-dependent shrinkage-induced curvature 71

Example 3.4 72 Crack control 75 3.7.1 General 75 3.7.2 Simpliﬁed code-oriented approaches for ﬂexural crack control 76 3.7.2.1 3.7.2.2 3.7.2.3 3.7.2.4 3.7.2.5

3.7.3

Gergely and Lutz 76 Frosch 77 Eurocode 2 – 1992 77 Eurocode 2 – 2004 77 ACI 318-08 79

Example 3.5 79 Tension chord model for ﬂexural cracking in reinforced concrete 83

37

Contents

vii

Example 3.6 87 Example 3.7 89 3.7.4 Model for direct tension cracking in restrained reinforced concrete 91 Example 3.8 95 3.8 References 96

4 Uncracked sections – axial loading

99

4.1 4.2

Preamble 99 The effective modulus method 100 4.2.1 Formulation 100 4.2.2 Example application (EMM) 101 Example 4.1 103 4.3 The principle of superposition – step-by-step method (SSM) 105 4.3.1 Formulation 105 4.3.2 Example application (SSM) – Approach 1 108 4.3.2.1 4.3.2.2

At ﬁrst loading (t = τ0 ) 108 At the end of the j-th time step (i.e. t = τj ) 108

Example 4.2 110 Example application (SSM) – Approach 2 114 Example 4.3 117 The age-adjusted effective modulus method (AEMM) 119 4.4.1 Formulation 119 4.4.2 Example application (AEMM) – Approach 1 121 4.4.3 Determination of the ageing coefﬁcient 122 Example 4.4 125 4.4.4 Example application (AEMM) – Approach 2 127 Example 4.5 128 The rate of creep method (RCM) 128 4.5.1 Formulation 128 4.5.2 Discussion 130 4.5.3 Example application (RCM) 130 Example 4.6 132 Comparison of methods of analysis 133 References 136 4.3.3

4.4

4.5

4.6 4.7

5 Uncracked sections – axial force and uniaxial bending 5.1 5.2 5.3

Introductory remarks 137 Overview of cross-sectional analysis 137 Short-term analysis of reinforced or prestressed concrete cross-sections 138 Example 5.1 143 Example 5.2 147

137

viii Contents 5.4

5.5

5.6

5.7

5.8

Long-term analysis of reinforced or prestressed concrete cross-sections using the age-adjusted effective modulus method (AEMM) 151 Example 5.3 157 Example 5.4 161 Long-term analysis of reinforced and prestressed cross-sections using the step-by-step procedure 164 Example 5.5 169 Example 5.6 174 Composite steel-concrete cross-sections 180 Example 5.7 182 Example 5.8 187 Composite concrete-concrete cross-sections 189 5.7.1 Short-term analysis 190 5.7.2 Time analysis – AEMM 192 Example 5.9 194 5.7.3 Time analysis – SSM 200 Example 5.10 203 References 223

6 Uncracked sections – axial force and biaxial bending

224

6.1 6.2

Introduction 224 Short-term analysis 226 Example 6.1 233 Example 6.2 236 Example 6.3 240 6.3 Long-term analysis using the age-adjusted effective modulus method (AEMM) 244 Example 6.4 248 Example 6.5 251 6.4 Long-term analysis using the step-by-step method 256

7 Cracked sections 7.1 7.2

Introductory remarks 260 Short-term analysis 265 7.2.1 Axial force and uniaxial bending 266 Example 7.1 271 Example 7.2 275 7.2.2 Axial force and biaxial bending 278 7.3 Time-dependent analysis (AEMM) 279 7.3.1 Axial force and uniaxial bending 279 Example 7.3 280 Example 7.4 285 7.3.2 Axial force and biaxial bending 288

260

Contents 7.4

ix

Short- and long-term analysis using the step-by-step method 288 7.4.1 Axial force and uniaxial bending 288 7.4.1.1 7.4.1.2

Instantaneous analysis 288 Time analysis 290

7.4.2 Axial force and biaxial bending 291 7.5 References 292

8 Members and structures 8.1 8.2

8.3

8.4

8.5

8.6

8.7 8.8

Introductory remarks 293 Deﬂection of statically determinate beams 293 8.2.1 Deﬂection and axial shortening of uncracked beams 293 Example 8.1 294 8.2.2 Control of deﬂection using non-prestressed reinforcement 297 8.2.3 Deﬂection and axial shortening of cracked beams 301 Example 8.2 302 Statically indeterminate beams and slabs 305 8.3.1 Discussion 305 8.3.2 Determination of redundants 306 Example 8.3 308 Example 8.4 310 8.3.3 Effects of deformation or settlement at the supports 316 Example 8.5 317 8.3.4 Further effects of creep in prestressed construction 320 Example 8.6 323 Two-way slab systems 324 8.4.1 Discussion 324 8.4.2 Slab deﬂection models 325 8.4.3 Two-way edge-supported slabs 326 Example 8.7 327 8.4.4 Flat slabs 330 Example 8.8 331 Slender reinforced concrete columns 335 8.5.1 Discussion 335 8.5.2 An iterative method of analysis 336 Example 8.9 337 Temperature effects 340 8.6.1 Introduction 340 8.6.2 Temperature distributions 341 8.6.3 Temperature analysis of cross-sections 341 Example 8.10 344 8.6.4 Temperature effects in members and structures 347 Example 8.11 347 Concluding remarks 349 References 349

293

x Contents

9 Stiffness method and ﬁnite-element modelling 9.1 9.2 9.3 9.4 9.5 9.6

9.7

9.8

351

Introduction 351 Overview of the stiffness method 351 Member loads 354 Example 9.1 356 Time analysis using AEMM 361 Example 9.2 363 Time analysis using SSM 368 Example 9.3 368 Time analysis using the ﬁnite-element method 376 9.6.1 Load vector to account for time effects using the AEMM 380 9.6.2 Load vector to account for time effects using the SSM 381 9.6.3 Remarks on the consistency requirements for ﬁnite elements 381 Example 9.4 383 Analysis of cracked members 387 9.7.1 Approach 1 387 9.7.2 Approach 2 389 References 389

Appendix A Analytical formulations – Euler-Bernoulli beam model

391

A.1 A.2 A.3 A.4

Introduction 391 Kinematic model 392 Weak formulation (global balance condition) 393 Finite element formulation 396 A.4.1 Age-adjusted effective modulus method 397 A.4.2 Step-by-step method 403 A.5 Strong formulation (local balance condition) 406 A.5.1 Instantaneous analysis 407 A.5.1.1 A.5.1.2 A.5.1.3

A.5.2

Age-adjusted effective modulus method (AEMM) 413 A.5.2.1 A.5.2.2

A.5.3

Index

Equivalent nodal actions at time τk 414 Post-processing of the solution at time τk 415

Step-by-step method (SSM) 417 A.5.3.1 A.5.3.2

A.6

Stiffness matrix 408 Equivalent nodal actions for member loads 411 Post-processing of the instantaneous solution 412

Equivalent nodal actions at time τk 422 Post-processing of the solution at time τi 423

References 423

424

Preface

In the design of concrete structures, the two main design objectives are strength and serviceability. A structure must be strong enough and sufﬁciently ductile to resist, without collapsing, the overloads and environmental extremes that may be imposed on it. It must also perform satisfactorily under the day-to-day service loads without deforming, cracking or vibrating excessively. This book is concerned with the serviceability of concrete structures, in particular the prediction of instantaneous and time-dependent deformation under in-service conditions. The factors that most affect structural behaviour at the serviceability limit states are considered in considerable depth, including cracking of the tensile concrete, tension stiffening, and the timedependent deformations caused by creep and shrinkage of the concrete. The prediction of the ﬁnal deformation of a concrete structure, and the ﬁnal extent and width of cracks, are perhaps the most uncertain and least well-understood aspect of structural design. The long-term behaviour of the structure depends primarily on the deformational characteristics of the concrete, including its creep and shrinkage characteristics, and these are highly variable, depending not only on the mix proportions and types of cement and aggregates, but also on the local environment and the load history. In most undergraduate civil and structural engineering courses, the effects of concrete creep and shrinkage on structural behaviour are treated superﬁcially, with only the simpliﬁed code-oriented procedures for deﬂection and crack control being presented. The same is true of most books on the design of concrete structures. Failure to recognise and quantify the non-linear effects of cracking, creep and shrinkage is a common cause of serviceability failure. Creep and shrinkage of concrete and their effects on structural behaviour have been actively researched for over 100 years. Much has been written on the subject and many outstanding contributions have been made. However, much of the information and many of the analytical procedures that have been developed are not, in general, known or used by the profession. Structural designers often rely on the simpliﬁed procedures in codes of practice to estimate service load behaviour, and this often oversimpliﬁes the problem and can be unreliable. This book is an attempt to provide practising engineers and post-graduate students with a practical and useful treatment of the serviceability analysis of concrete structures. For this purpose, most sections included in each chapter are self-contained so that they can be read independently from the rest of the book. The analytical techniques are illustrated by numerous worked examples. In Chapter 1, an introductory discussion of concrete creep and shrinkage and their effects on the deformation of concrete structures is presented, while typical

xii Preface material properties and a simple procedure for estimating the creep and shrinkage characteristics of concrete are provided in Chapter 2. No attempt has been made to provide a detailed description of the mechanisms of creep and shrinkage or the factors affecting them. The material properties and material constitutive relationships are only of interest insofar as they affect the methods of structural analysis. Chapter 3 contains a qualitative discussion of structural behaviour at service loads and the simpliﬁed methods for the control of deﬂection and cracking contained in several of the major codes of practice are presented and critically reviewed, including ACI318-08, Eurocode 2 and the Australian Standard AS3600-2009. Alternative and more reliable procedures for deﬂection calculation and crack control are also provided. Chapters 4–7 deal with the time-dependent analysis of cross-sections, exploring various procedures for predicting the gradual change of strain and curvature with time and the gradual redistribution of stress between the concrete and the bonded steel reinforcement. Chapter 4 examines cross-sections loaded in axial compression. Chapter 5 considers a wide range of uncracked reinforced, prestressed and composite cross-sections carrying axial force and uniaxial bending. Chapter 6 deals with uncracked cross-sections subject to combined axial force and biaxial bending. Cracked cross-sections subjected to axial force and bending are analysed in Chapter 7. In Chapter 8, a range of different structural applications are considered, drawing on the cross-sectional analyses in Chapters 4–7 and the treatment of tension stiffening and cracking in Chapter 3. The techniques described and illustrated may be extended readily to include a wide range of additional structural applications. The procedures are not daunting and require little more than an elementary background in mechanics and structural analysis. Chapter 9 illustrates how the time-dependent effects of creep and shrinkage can be readily included in the computer analysis of structures using the stiffness and the ﬁniteelement methods. These have been described and applied considering the common Euler–Bernoulli beam model as a case study, but the approach is general and can be extended to more complex models. The analytical formulations required to implement the computer analysis of Chapter 9 are presented in Appendix A. It is hoped that this book will provide structural engineers not only with useful analytical tools to predict and control in-service performance, but also with a clearer picture of the interaction between concrete and reinforcement at service loads and a better understanding of why concrete structures behave as they do. Raymond Ian Gilbert and Gianluca Ranzi Sydney, 2010.

Acknowledgements

The authors acknowledge the support given by their respective institutions and by the Australian Research Council through its Discovery and Linkage schemes and the award of an ARC Australian Professorial Fellowship for the period 2005 to 2010 to the ﬁrst author. Thanks are also extended to Associate Professor Graziano Leoni and Dr Andrew Kilpatrick for their comments on the drafts of each chapter and to Associate Professor Rob Wheen for providing the cover photograph of the Anzac Bridge during construction.

Notation and sign convention

All symbols are deﬁned in the text where they ﬁrst appear. The more frequently used symbols and those that appear throughout the book are listed below. It is assumed that tension is positive and compression is negative, and positive bending about a horizontal axis causes tension in the bottom ﬁbres of a cross-section. A, B, I

A c , B c , Ic Ae , Be , I e Ass , Bss , Iss Act As(i) , Ap(i) Ast , Asc b, bw b∗ C C(t, τ0 ) c D0 , D j , D k D d db ds(i) , dp(i) dn (=kd) do dref

area, ﬁrst moment of area, and second moment of area, respectively, calculated about the reference axis of the cross-section properties A, B and I of the concrete part of the cross-section properties A, B and I of the age-adjusted transformed cross-section properties A, B and I of the structural steel part of a composite cross-section area of tensile concrete in the tension chord (Eq. 3.45) areas of the ith layer of non-prestressed and prestressed steel, respectively areas of tensile and compressive steel on a reinforced section, respectively ﬂange width and web width of a T-section width of cross-section at the level of the centroid of the tensile reinforcement speciﬁc creep (also Celsius) speciﬁc creep at time t produced by a sustained unit stress ﬁrst applied at τ0 concrete cover to reinforcement matrices of cross-sectional rigidities at τ0 , τj and τk , respectively overall depth of a cross-section effective depth of the tensile reinforcement bar diameter depths to the i-th layer of the non-prestressed and prestressed steel, respectively depth to the neutral axis on a fully-cracked cross-section depth from extreme compressive ﬁbre to the centroid of the outermost layer of tensile reinforcement depth of reference axis below the top ﬁbre of the cross-section

Notation and sign convention xv Ec , Es , Ep , Ess Ec,j Ee , Ee Ee,j,i e eAB eL f cr,j , f cr,k f set,j , f set,k f p,init f sh,j , f sh,k F F 0 , Fj , F k Fe,j,i Fe,0 fc , ft fc fcm , fcmi fct fct,f fji fp fst fy G, g Icr , Iuncr Ief Ig i, j, k h J J(t, τ0 ) Jj,i K

elastic moduli of concrete, non-prestressed steel, prestressed steel, and structural steel, respectively elastic modulus of concrete at time τj effective modulus of concrete (Eq. 4.3) and age-adjusted effective modulus of concrete (Eq. 4.35), respectively effective modulus of concrete at time τj due to a stress ﬁrst applied at τi eccentricity; base of the natural logarithm axial deformation of member AB axial shortening of a column of length, L vectors of actions at times τj and τk , respectively, accounting for creep during previous time periods vectors of corrected internal actions to be used at times τj and τk , respectively, when a new element is added to a cross-section vector of initial prestressing forces vectors of actions at times τj and τk , respectively, accounting for shrinkage during previous time periods ﬂexibility matrix matrices relating strain to internal actions on cross-section at τ0 , τj and τk , respectively creep factor at time τj for a stress applied at τi (Eq. 4.26b) age-adjusted creep factor (Eq. 4.46) strength of concrete in compression and in tension, respectively characteristic strength of concrete in compression mean concrete cylinder strength and mean concrete in-situ strength, respectively uniaxial tensile strength of concrete characteristic ﬂexural tensile strength of concrete (modulus of rupture) a ﬂexibility coefﬁcient (the displacement at release j due to a unit value of the ith redundant force) breaking strength of the prestressing steel steel stress on a cracked section corresponding to a crack width of w∗ yield stress of the non-prestressed steel dead load (kN) and dead load per unit area (kPa), respectively second moments of area of the fully-cracked and uncracked transformed cross-section about the centroidal axis, respectively effective second moment of area after cracking second moment of area of gross cross-section about centroidal axis integers slab thickness creep function creep function at time t for concrete ﬁrst loaded at τ0 (Eq. 1.10) creep function at time τj due to a stress ﬁrst applied at τi structural stiffness matrix

xvi Notation and sign convention kd kcs ke k1 , k2 , k3 , k4 , k5 L, Lx , Ly ln ef M Mcr Ms∗ Mu Mxe , Mye mc mp , ms Nc,0 , Ns,0 , Np,0 Nc,k , Ns,k , Np,k Ncr Ne , Me Ni,0 , Mi,0 Ni,k , Mi,k Nsus , Msus n ne , ne ne,j,i P P Pcr Pp,init p Q, q R RA,0 , RB,0 , RI,0 RA,k , RB,k , RI,k Rb RP RR re,k ri,k S

depth to neutral axis from extreme compressive ﬁbre long-term to short-term deﬂection multiplication factor element stiffness matrix factors describing the magnitude and rate of development of creep and shrinkage span of a beam or length of a column orthogonal span lengths for two-way slabs the natural logarithm the effective span (the lesser of the centre-to-centre distance between the supports and the clear span plus the member depth) moment cracking moment design in-service moment at the critical cross-section ultimate ﬂexural strength applied moments about the x- and y-axes, respectively number of layers of concrete in a discretised cross-section number of layers of tendons and non-prestressed reinforcement on a cross-section internal forces resisted by concrete, reinforcement and tendons at time τ0 , respectively internal forces resisted by concrete, reinforcement and tendons at time τk , respectively restraining force after direct tension cracking external axial force and moment applied to a cross-section internal axial force and moment on a cross-section at time τ0 internal axial force and moment on a cross-section at time τk sustained axial force and moment applied to a cross-section modular ratio (Es /Ec ) effective and age-adjusted effective modular ratios (Es /Ee , Es / Ee ), respectively effective modular ratio (Es /Ee,j,i ) vector of nodal loads for whole structure axial load; also prestressing force cracking load initial prestressing force prior to transfer vector of nodal loads for element live load (kN) and live load per unit area (kPa), respectively design relaxation force in the prestressing steel cross-sectional rigidities at time τ0 cross-sectional rigidities at time τk basic relaxation vector of reactions caused by loads on the primary structure vector of redundant forces vector of external actions at time τk vector of internal actions at time τk ﬁrst moment of area of the steel reinforcement about the centroid of the section

Notation and sign convention xvii s sb smax so s∗ T t th U u ue v vcx vmy vsus W w w∗ ws x y yn,0 ys , y p Z z α α1 , α2 , α3 β ε, κ δ δB ε εtop , εbtm ε˙ εcr εcr (t, τ0 ) ∗ εcr εe εr εr0 , εrk εp

spacing between cracks in the tensile zone maximum bar spacing maximum crack spacing immediately after loading distance over which the stresses vary on each side of a direct tension crack ﬁnal maximum crack spacing temperature; also tensile force time hypothetical thickness vector of nodal displacements for whole structure vector of nodal displacements for element portion of section perimeter exposed to the atmosphere deﬂection deﬂection of a column strip in the x-direction deﬂection of a middle strip in the y-direction deﬂection due to sustained loading wind load crack width; also uniformly distributed load maximum design crack width uniformly distributed sustained service load reference axis transverse distance from the reference axis in the plane of the section distance of neutral axis from x-axis on a cracked section at time τ0 y-coordinates of steel reinforcement and tendons, respectively section modulus direction of member axis coefﬁcient of thermal expansion; also a parameter to account for cracking and reinforcement on the change in deformation due to creep (Eqs 3.32) coefﬁcients associated with creep and shrinkage models (Sections 2.1.4 and 2.1.5) tension stiffening coefﬁcient to account for duration of loading an increment or a change change in strain and curvature with time, respectively lateral displacement of a slender column settlement at support B strain strains at the top and bottom ﬁbres of a cross-section, respectively rate of change of strain with time (dε/dt) creep strain creep strain at time t due to a stress ﬁrst applied at τ0 ﬁnal creep strain at time inﬁnity instantaneous (elastic) strain strain at reference axis strain at reference axis at time τ0 and at time τk , respectively strain in the prestressing steel

xviii Notation and sign convention εp,init εp.rel,k εs εsh εshd εshe ∗ εsh εT θ θM θNA κ κcr , κuncr κ0 , κk κsh κx , κy λr R λ 1 , λ2 , λ3 με ρ, ρ ρw , ρcw σ σc , σs σc,0 , σs,0 σc,k , σs,k σcs σp,init σ˙ σp(i) , σs(i) σst1 σtop τ τ0 τb τd τi τk ϕ ϕ(t, τ0 ) ϕbasic ϕj,i

initial strain in the prestressing steel before transfer relaxation strain in the prestressing steel at time τk strain in the steel reinforcement shrinkage strain drying shrinkage strain endogenous (chemical plus thermal) shrinkage strain ﬁnal shrinkage strain at time inﬁnity temperature component of strain slope angle between moment axis and the x-axis angle between the neutral axis and the x-axis curvature curvatures on fully-cracked and uncracked cross-section, respectively curvatures at time τ0 and at time τk , respectively curvature induced by shrinkage curvature with respect to the x-axis and y-axis, respectively reduced relaxation in the prestressing steel accounting for creep and shrinkage factors affecting bond stress microstrain (10−6 ) tensile reinforcement ratio Ast /bd (or Ast /Ac ) and compressive reinforcement ratio, Asc /bd, respectively or; also, density web reinforcement ratio for the tensile steel ((Ast + Apt )/bw d) and compressive steel (Asc /bw d), respectively the sum of stress concrete and steel stresses, respectively initial concrete and steel stresses, respectively, at ﬁrst loading, τ0 ﬁnal concrete and steel stresses, respectively, at time τk shrinkage-induced tensile stress in the concrete initial stress in the prestressing steel prior to transfer rate of change of concrete stress with time, dσ /dt stresses in the i-th layer of prestressed and non-prestressed steel, respectively tensile steel stress at a crack concrete stress at top ﬁbre of cross-section time instant; also shear stress age at ﬁrst loading bond shear stress age at the commencement of drying i-th time instant ﬁnal time instant at the end of the period of the time analysis creep coefﬁcient creep coefﬁcient at time t for concrete loaded at τ0 basic creep coefﬁcient creep coefﬁcient at time τj due to a stress ﬁrst applied at τi

Notation and sign convention xix ϕ˙ ϕp ϕ∗ χ χ(t, τ0 ) χ∗ ψ1 , ψ2 ζ ∞

rate of change of the creep coefﬁcient with time, dϕ/dt creep coefﬁcient for the prestressing steel ﬁnal creep coefﬁcient at time inﬁnity ageing coefﬁcient ageing coefﬁcient at time t for concrete ﬁrst loaded at τ0 ﬁnal ageing coefﬁcient at time inﬁnity short- and long-term serviceability load factors distribution factor to account for tension stiffening (Eq. 3.24) inﬁnity

1

Time-dependent deformation

1.1 Background When a concrete specimen is subjected to load, its response is both immediate and timedependent. Under sustained load, the deformation of a specimen gradually increases with time and eventually may be many times greater than its initial value. In order to satisfy the design objective of serviceability in a structural design, accurate and reliable predictions of the instantaneous and time-dependent deformation of the concrete structure are required. If the temperature and stress remain constant, the gradual development of strain with time is caused by creep and shrinkage. Creep strain is produced by sustained stress, while shrinkage strain is independent of stress. These inelastic and timedependent strains cause increases in deformation and curvature, losses of prestress and redistribution of stresses and internal actions. Creep and shrinkage are often responsible for excessive deﬂection at service loads. Creep frequently causes excessive camber and/or shortening in prestressed members. In addition, restraint to shrinkage may cause time-dependent cracking that could lead to serviceability or durability failures. To accurately and efﬁciently predict these effects, the following two basic prerequisites are necessary: (i) reliable data for the creep and shrinkage characteristics of the particular concrete mix; and (ii) analytical and/or numerical procedures for the inclusion of these time effects in the analysis and design of the structure. A number of sources are available from which to obtain information on the properties of concrete (see Sections 2.1.2–2.1.5). However, a comparison of the data obtained from these sources indicates signiﬁcant differences. Laboratory tests may be undertaken to determine time-dependent material properties but this is often not a practical alternative. Designers seldom have the time or the inclination for longterm tests and then often cannot be sure that the concrete that has been tested in the laboratory is the same as that which will later be used in the structure. Even if testing is undertaken, the variability in the measured deformational properties of concrete is usually large. Coefﬁcients of variation of 20 per cent or more can be expected. To best

2 Time-dependent deformation account for the variability of material properties in structural design, probabilistic methods are required. However, existing design methods are usually deterministic and the inexact nature of the results of such procedures must be kept in mind. A number of analytical and numerical techniques are available for serviceability analysis and the design of reinforced and prestressed concrete structures. These range from simpliﬁed approaches for deﬂection and crack control contained in codes of practice, such as those presented and evaluated in Chapter 3, to the more reﬁned methods contained in Chapters 4–9. Each level of reﬁnement has its own set of simplifying assumptions and each has its advantages and disadvantages. Some are more suited to particular situations than others. Throughout the book, many worked examples are provided and a wide range of structural applications and situations are considered. The worked examples are also self-contained and may be read by practitioners who are more interested in using the ﬁnal equations rather than following their detailed derivations. However, for most applications, the mathematics associated with each analysis is quite straightforward and there are obvious advantages in understanding the development of the procedures. Methods of analysis that include the effects of creep and shrinkage in concrete structures are important in the design for serviceability. But perhaps even more importantly, such analyses can provide a clear picture of the interaction between concrete and steel and an otherwise unavailable insight into the mechanism of structural behaviour. A study of time effects can provide the structural designer with a far better feel for the task and a clearer understanding of why concrete structures behave as they do. 1.1.1 Concrete strain components At any time t, the total concrete strain ε(t) in an uncracked, uniaxially-loaded specimen consists of a number of components that include the instantaneous strain εe (t), creep strain εcr (t), shrinkage strain εsh (t) and temperature strain ε T (t). Although not strictly correct, it is usual to assume that all four components are independent and may be calculated separately and combined to obtain the total strain. When calculating the inservice behaviour of a concrete structure at constant temperature, it is usual to express the concrete strain at a point as the sum of the instantaneous, creep and shrinkage components: ε(t) = εe (t) + εcr (t) + εsh (t)

(1.1)

The strain components in a drying specimen held at constant temperature and subjected to a constant sustained compressive stress σc0 ﬁrst applied at time τ 0 are illustrated in Fig. 1.1. Immediately after the concrete sets or at the end of moist curing (t = τd in Fig. 1.1), shrinkage strains begin to develop and continue to increase at a decreasing rate. On the application of stress, a sudden jump in the strain diagram (instantaneous or elastic strain) is followed by an additional gradual increase in strain due to creep. The prediction of the time-dependent behaviour of a concrete member requires the accurate prediction of each of these strain components at critical locations. This requires knowledge of the stress history, in addition to accurate data for the

Time-dependent deformation 3

Total strain ecr(t) – creep ee(t) − instantaneous

esh(t) − shrinkage

0 td

t0

Time, t

t0

Time, t

Stress sc0

0

Figure 1.1 Concrete strain components under sustained load.

material properties. The stress history depends on both the applied load and the boundary conditions of the member. It has been common practice in previous studies of the deformation of concrete to distinguish between creep problems and relaxation problems. Creep problems are those in which the gradual increase in strain under a sustained stress is calculated. Relaxation problems are those in which the total strain is held constant with time and the gradual change in stress is calculated. Creep and relaxation problems differ only in their boundary conditions. Both involve the estimation of the individual strain components in Eq. 1.1. Relaxation problems have the additional constraint that the sum of the change of each strain component within any time interval is zero, that is, εe (t) + εcr (t) + εsh (t) = 0. When the total strain is held constant, the change of stress with time (relaxation) is simply the result of the gradual development of creep and shrinkage and the consequent equal and opposite change in the instantaneous strain. If creep and shrinkage increase with time, then the instantaneous strain εe (t) must decrease. There is little to be gained from separate studies of creep and relaxation type problems. In fact, in reinforced concrete structures, it is uncommon to ﬁnd situations which fall neatly into the categories of either creep or relaxation problems. Concrete is almost never free to deform without some form of restraint. Reinforcement provides internal restraint to creep and shrinkage, while real support conditions often provide signiﬁcant external restraint. On the other hand, a member is rarely restrained so completely that no deformation of the concrete is possible. Real problems often involve elements of both creep and relaxation, and fall between these two extremes. For the time analysis of concrete structures, attention should be focused squarely on the problem of establishing suitable constitutive relationships for concrete that can be used

4 Time-dependent deformation in the analysis of practical problems for the determination of the strain components of Eq. 1.1 at any point in the structure. 1.1.2 Typical concrete strain magnitudes It is important from the outset to ﬁrmly establish the signiﬁcance of each of the concrete strain components and their order of magnitude in typical in-service situations. Consider a point in a concrete specimen subjected to a constant, sustained compressive stress σ c0 applied at time τ0 and equal to 40 per cent of the characteristic compressive strength of concrete, i.e. σc0 = 0.4 fc . In properly designed concrete structures, concrete stresses rarely exceed this level under typical service loads. The instantaneous strain that occurs immediately upon application of the stress may be considered to be elastic at low stress levels, and therefore: εe (t) =

σc0 Ec (τ0 )

(1.2)

Information on the time-varying nature of the elastic modulus for concrete, Ec (t), is given in Section 2.1.3. However, for comparison between the order of magnitude of each of the strain components in Eq. 1.1, the elastic modulus may be taken as constant with time and approximately equal to 1000 fc . In this case, therefore, the elastic strain is approximated by: εe ≈

−0.4 fc = −0.0004 = −400 με 1000 fc

where the negative sign indicates that the applied stress and elastic strain are compressive. Under normal conditions, the ﬁnal creep strain at time inﬁnity εcr (∞) (denoted here ∗ ) that is produced by a constant sustained stress of this magnitude is usually as εcr between 1.5 and 4.0 times the initial elastic strain. The higher end of this range is for low-strength concrete loaded at early ages and at a low relative humidity. A typical ﬁnal creep strain for structural concrete subjected to constant stress of this level is 2.5 εe and, for this case, ∗ ≈ 2.5 εe = −1000με εcr ∗ ) depends on The ﬁnal shrinkage strain at time inﬁnity εsh (∞) (denoted here as εsh the concrete composition, the environment and the size and shape of the specimen. For concrete elements in building structures, a typical value is: ∗ ≈ −600 με εsh

The thermal strain produced by a change in temperature T = T − T0 is calculated from: T εT =

α dT T0

(1.3)

Time-dependent deformation 5 where T0 is the initial temperature and α is the coefﬁcient of thermal expansion that is approximately 10 × 10−6 /◦ C (but actually depends on temperature and moisture content). For a 20◦ C change in temperature, the change in thermal strain is approximately α T = 200 με. If the specimen under consideration is held at constant temperature, the total concrete strain at time inﬁnity (which may be considered as several years after loading) is: ∗ ∗ ε∗ = εe + εcr + εsh ≈ −400 − 1000 − 600 = −2000 με

(1.4)

Thus the magnitude of the ﬁnal strain is about ﬁve times the magnitude of the instantaneous elastic strain. It must be emphasised that the magnitudes of the creep and shrinkage considered here are typical and not extreme values. Therefore, when calculating the deformation of concrete structures, time effects must be included in a rational and systematic way. Elastic analyses that ignore the effects of creep and shrinkage may grossly underestimate ﬁnal deformations and, in the design of concrete structures for serviceability, are of little value.

1.2 Creep of concrete 1.2.1 Creep mechanisms and inﬂuencing factors When concrete is subjected to a sustained stress, creep strain develops gradually with time as shown in Fig. 1.1. Creep increases with time at a decreasing rate. In the period immediately after initial loading, creep develops rapidly, but the rate of increase slows appreciably with time. Creep is generally thought to approach a limiting value as the time after ﬁrst loading approaches inﬁnity. About 50 per cent of the ﬁnal creep develops in the ﬁrst 2–3 months and about 90 per cent after 2–3 years. After several years under load, the rate of change of creep with time is very small. Throughout this book, creep and shrinkage are treated as separate and independent phenomena. In reality, this is not the case. Creep is signiﬁcantly greater when accompanied by shrinkage. In a loaded specimen that is in hygral equilibrium with the ambient medium (i.e. no drying), the time-dependent deformation caused by stress is known as basic creep. The additional creep that occurs in a drying specimen is sensibly known as drying creep. Creep is usually calculated as the difference between the total time-dependent deformation of a loaded specimen and the shrinkage of a similar unloaded specimen. Creep is treated here as the time-dependent deformation in excess of shrinkage. Creep of concrete originates in the hardened cement paste that consists of a solid cement gel containing numerous capillary pores. The cement gel is made up of colloidal sheets of calcium silicate hydrates separated by spaces containing absorbed water. Creep is thought to be caused by several different and complex mechanisms not yet fully understood (Refs 1–7). Neville et al. (Ref. 4) identiﬁed the following mechanisms for creep: (i) sliding of the colloidal sheets in the cement gel between the layers of absorbed water – viscous ﬂow;

6 Time-dependent deformation (ii) expulsion and decomposition of the interlayer water within the cement gel – seepage; (iii) elastic deformation of the aggregate and the gel crystals as viscous ﬂow and seepage occur within the cement gel – delayed elasticity; (iv) local fracture within the cement gel involving the breakdown (and formation) of physical bonds – microcracking; (v) mechanical deformation theory; and (vi) plastic ﬂow. Recent research relates the creep response to the packaging density distributions of calcium-silicate-hydrates (Ref. 7). At high stress levels, additional deformation occurs due to the breakdown of the bond between the cement paste and aggregate particles. Further references on creep mechanisms can be found in Refs 1 and 8. Many factors inﬂuence the magnitude and rate of development of creep. Some are properties of the concrete mix, while others depend on the environmental and loading conditions. In general, the capacity of the concrete to creep decreases as the concrete strength increases. For a particular stress level, creep in higher-strength concrete is less than that in lower-strength concrete. An increase in either the aggregate content or the maximum aggregate size reduces creep, as does the use of a stiffer aggregate type. Creep also decreases as the water-to-cement ratio is reduced. Creep also depends on the environment. It increases as the relative humidity decreases. Creep is also greater in thin members with large surface-area-to-volume ratios, such as slabs. However, the dependence of creep on both the relative humidity and the size and shape of the specimen decreases as the concrete strength increases. Near the surface of a member, creep takes place in a drying environment and is therefore greater than in regions remote from a drying surface. In addition to the relative humidity, creep is dependent on the ambient temperature. A rise in temperature increases the deformability of the cement paste and accelerates drying, and thus increases creep. The dependence of creep on temperature is more pronounced at elevated temperatures and is far less signiﬁcant for temperature variations between 0◦ C and 20◦ C. However, creep in concrete at a mean temperature of 40◦ C is perhaps 25 per cent higher than that at 20◦ C (Ref. 9). In addition to the environment and the characteristics of the concrete mix, creep depends on the loading history, in particular the magnitude and duration of the stress and the age of the concrete when the stress was ﬁrst applied. The age of the concrete, τ 0 , when the stress was ﬁrst applied has a marked inﬂuence on the ﬁnal magnitude of creep. Concrete loaded at an early age creeps more than concrete loaded at a later age. Concrete is therefore a time-hardening material, although even in very old concrete the tendency to creep never entirely disappears (Ref. 10). When the sustained concrete stress is less than about 0.5 fc , creep is approximately proportional to the stress and is known as linear creep. At higher stress levels creep increases at a faster rate and becomes non-linear with respect to stress. This nonlinear behaviour of creep at high stress levels is thought to be related to an increase in micro-cracking. Compressive stresses rarely exceed 0.5 fc in concrete structures at service loads, and creep may be taken as proportional to stress in most situations in the design for serviceability. In this book, the effects of non-linear creep at high stress levels are not examined.

Time-dependent deformation 7 1.2.2 Creep components To best understand the physical nature of creep and to describe its characteristics, creep strain is often subdivided into several components. In Fig. 1.2a, the creep strain produced by the compressive stress history of Fig. 1.2b is shown. Under sustained stress σo , creep increases at a decreasing rate. When the stress is removed at time τ1 , there is no sudden change in creep strain, but a gradual reduction occurs with time as shown. There is of course a sudden change in the total strain at τ1 due to the elimination of instantaneous strain. A portion of the creep strain is recoverable, while a usually larger portion is irrecoverable or permanent. The recoverable part of creep is often referred to as the delayed elastic strain, εcr.d (t). This delayed elasticity is thought to be caused by the elastic aggregate acting on the viscous cement paste after the applied stress is removed. If a concrete specimen is unloaded after a long period under load, the magnitude of the recoverable creep is in the order of 40–50 per cent of the elastic strain (between 10 and 20 per cent of the total creep strain). Although the delayed elastic strain is observed only as recovery when the load is removed, it is generally believed to be of the same magnitude under load and to develop rapidly in the period immediately after loading. Rüsch et al. (Ref. 8) suggest that the shape of the delayed elastic strain curve is independent of the age or dimensions of the specimen and is unaffected by the composition of the concrete. The majority of creep strain is irrecoverable and is often referred to as ﬂow, ε cr.f (t). The ﬂow component of creep is sometimes further subdivided into rapid initial ﬂow, εcr.ﬁ (t), that occurs in the ﬁrst 24 hours after loading, and the remaining ﬂow that develops gradually with time (Ref. 9). The rapid initial ﬂow is irrecoverable and highly dependent on the age at ﬁrst loading, that is, on the degree of hydration. The younger concrete is when ﬁrst loaded, the higher ε cr.ﬁ (t). The remaining ﬂow that occurs after the ﬁrst day under load is dependent on the relative humidity and, as discussed earlier, may be divided into a basic ﬂow component εcr.fb (t) and a drying ﬂow component εcr.fd (t). The drying ﬂow is the additional irrecoverable creep that occurs when the specimen is loaded in a drying environment. The basic ﬂow ε cr.fb (t) depends on the composition of the concrete mix (aggregate type, size and quantity, concrete strength, etc.) and the age of the concrete at the time of loading. The drying ﬂow εcr.fd (t) depends on the moisture content and gradient, and the size and shape of the specimen. In structural analysis, it is unusual to subdivide the ﬂow component of creep into all of these sub-components. However, consideration of the recoverable and irrecoverable Creep strain

Recoverable creep, −ecr.d (t1)

ecr(t) ecr.f

Irrecoverable creep, ecr.f (t1) +ecr.d (a)

t0

t1

Time

t0

t1

Time

Stress s0 (b)

Figure 1.2 Recoverable and irrecoverable creep components.

8 Time-dependent deformation components of creep (i.e. the delayed elastic and ﬂow components, respectively) is appropriate and necessary if concrete is subjected to a time-varying stress history. 1.2.3 Effects of ageing In the previous sections, we saw that all sub-components of creep are affected to some extent by the degree of hydration, i.e. the age of the concrete at the time of ﬁrst loading, τ . Fig. 1.3 shows the effect of age at ﬁrst loading on the creep–time curves of identical specimens ﬁrst loaded at ages τ 0 , τ 1 and τ 2 . Although not proven, it is usually assumed that the creep strain εcr (t, τ ) approaches ∗ (τ ). All else being equal: a limiting value as time approaches inﬁnity, i.e. εcr (∞, τ ) = εcr ∗ ∗ (τi ) > εcr (τj ) εcr

τi < τj

provided

(1.5)

This time-hardening or ageing of concrete complicates the prediction of creep strain under time-varying stress histories. 1.2.4 The creep coefﬁcient, ϕ(t,τ ), and the creep function, J(t, τ ) The capacity of concrete to creep is usually measured in terms of the creep coefﬁcient, ϕ(t,τ ). In a concrete specimen subjected to a constant sustained compressive stress, σc (τ ), ﬁrst applied at age τ , the creep coefﬁcient at time t is the ratio of the creep strain to the instantaneous strain and is given by: ϕ(t, τ ) =

εcr (t, τ ) εe (τ )

(1.6)

Therefore, the creep strain at time t caused by a constant sustained stress σc (τ ) ﬁrst applied at age τ is: εcr (t, τ ) = ϕ(t, τ ) εe (τ ) = ϕ(t, τ )

σc (τ ) Ec (τ )

(1.7)

Creep strain, ecr(t,t)

where Ec (τ ) is the elastic modulus at time τ . For concrete subjected to a constant sustained stress, knowledge of the creep coefﬁcient allows the rapid determination of the creep strain at any time.

e*cr (t0) e*cr (t1) * ecr (t2)

t0

t1

t2

Time

Figure 1.3 Effect of age at ﬁrst loading on creep strains.

Time-dependent deformation 9 Since both the creep and instantaneous strain components are proportional to stress for compressive stress levels less than about 0.5 fc , the creep coefﬁcient ϕ(t,τ ) is a pure time function and is independent of the applied stress. The creep coefﬁcient increases with time at an ever-decreasing rate. As time approaches inﬁnity, the creep coefﬁcient ∗ (τ )/ε (τ ) that usually falls within is assumed to approach a ﬁnal value ϕ ∗ (τ ) = εcr e the range 1.5–4.0. This ﬁnal creep coefﬁcient is a useful measure of the capacity of concrete to creep. Since creep strain depends on the age of the concrete at the time of ﬁrst loading, so too does the creep coefﬁcient. A family of creep coefﬁcient versus time curves may be drawn that are similar to the creep–time curves shown in Fig. 1.3. Another frequently used time function is known as speciﬁc creep, C(t,τ ), and is the proportionality factor relating stress to linear creep, i.e.: εcr (t, τ ) = C(t, τ ) σc (τ )

or C(t, τ ) =

εcr (t, τ ) σc (τ )

(1.8)

C(t, τ ) is the creep strain at time t produced by a sustained unit stress ﬁrst applied at age τ . The relationship between the creep coefﬁcient and speciﬁc creep can be obtained from Eqs 1.6 and 1.8: ϕ(t, τ ) = C(t, τ ) Ec (τ )

(1.9)

The sum of the instantaneous and creep strains at time t produced by a sustained unit stress applied at τ is deﬁned as the creep function, J(t, τ ), and is given by: J (t, τ ) =

1 1 + C(t, τ ) = [1 + ϕ(t, τ )] Ec (τ ) Ec (τ )

(1.10)

The stress-produced strains (i.e. the instantaneous plus creep strains) caused by a constant sustained stress σ c (τ ) ﬁrst applied at age τ (also called the stress-dependent strains) may therefore be determined from: εe (t) + εcr (t, τ ) = J(t, τ )σc (τ ) =

σc (τ ) σc (τ ) [1 + ϕ(t, τ )] = Ec (τ ) Ee (t, τ )

(1.11)

where Ee (t, τ ) is known as the effective modulus and is given by: Ee (t, τ ) =

Ec (τ ) [1 + ϕ(t, τ )]

(1.12)

The variation with time of the creep strain caused by a constant sustained stress σc (τ0 ) (≡σ c0 ) is shown in Fig. 1.4. In the remainder of this book, the creep coefﬁcient and the creep function are used to mathematically deﬁne and quantify creep. 1.2.5 The principle of superposition Because the load-dependent strains in concrete at service loads are proportional to stress, the principle of superposition is frequently used to estimate the deformation

10 Time-dependent deformation sc(t)

ecr(t, t0)

sc(t0)

j(t, t0) sc(t0)/Ec(t0) t0 Time (a) Constant stress history

t0 Time (b) Creep strain versus time

Figure 1.4 Creep strain produced by a constant sustained stress.

caused by a time-varying stress history. The principle of superposition was ﬁrst applied to concrete by McHenry (Ref. 11) who stated that the strain produced by a stress increment applied at any time τ i is not affected by any stress applied either earlier or later. This principle is illustrated in Fig. 1.5. For increasing stress histories, such as that shown in Fig. 1.5c, the principle of superposition agrees well with experimental observations. The creep curve produced by the increasing stress history is assumed to be equal to the sum of the creep curves produced by each stress increment acting independently. However, for decreasing stress histories, the principle of superposition overestimates creep recovery, as shown in Fig. 1.5d. This can easily be seen when one divides creep into delayed elastic and ﬂow components. The principle of superposition incorrectly assumes that at any time t τ1 , the delayed elastic strain that develops between τ0 and τ1 , εcr.d (τ1 , τ0 ), is equal to the Curve (a)

ecr (t)

sc

j(t,t0) sc (t0 )/Ec(t0)

sc(t0)

(a)

t0

Time

t0

Time

ecr (t)

sc

Curve (b)

sc(t1) = sc(t0)

sc(t1)

j(t,t1) sc(t1)/Ec(t1)

(b)

t1

t1

Time

Time

ecr (t) sc 2sc(t0 )

Curve (c) = Curve (a) + Curve (b)

sc(t0 )

(c)

t0

t1

t0

Time

t1

Time

ecr (t)

Actual

sc sc(t0 )

(d)

Curve (d) = Curve (a) − Curve (b) t0

t1

Time

t0

t1

Time

Figure 1.5 The principle of superposition of creep strains.

Time-dependent deformation 11 creep strain at time t produced by σc (τ1 ) = σc (τ0 ) applied at τ1 (i.e. εcr (t, τ1 )). In fact, εcr.d (τ1 , τ0 ) is signiﬁcantly less than εcr (t, τ1 ). Nevertheless, for most practical purposes, the principle of superposition provides a good approximation of the time-dependent strains in concrete caused by a time-varying stress history. To illustrate the principle of superposition, consider the stress history shown in Fig. 1.6a consisting of two stress increments σ c (τ 0 ) and σ c (τ 1 ) applied at times τ 0 and τ 1 , respectively. In this case, two creep coefﬁcients ϕ(t, τ 0 ) and ϕ (t, τ 1 ) are required to determine the creep strain at any time t > τ 1 . Graphs of the two creep coefﬁcients versus time curves are shown in Fig. 1.6b and the corresponding creep function versus time curves are given in Fig. 1.6c. According to the principle of superposition, the total stress-dependent strain in concrete at time t (elastic plus creep strains) can be written as: εe (t) + εcr (t) = =

σc (τ0 ) σc (τ1 ) [1 + ϕ(t, τ0 )] + [1 + ϕ(t, τ1 )] Ec (τ0 ) Ec (τ1 ) 1 σc (τi ) i=0

Ec (τi )

[1 + ϕ(t, τi )]

(1.13)

where the argument τ has been eliminated from the elastic strain εe (t) and creep strain εcr (t) as the stress history varies with time. This notation is more appropriate for realistic time-varying stress histories and will be used throughout the remainder of the book. Eq. 1.13 can also be written in terms of creep functions as: εe (t) + εcr (t) = J(t, τ0 )σc (τ0 ) + J(t, τ1 )σc (τ1 ) =

1

J(t, τi )σc (τi )

(1.14)

i=0

The variations with time of the elastic and creep deformations are plotted in Fig. 1.7. A useful graphic interpretation of the elastic and creep deformations is shown in Fig. 1.8, where Figs 1.6a and 1.6c have been combined. The stress increments of Fig. 1.6a are plotted on the horizontal axis of Fig. 1.8b and Fig. 1.6c has been reproduced for ease of reference in Fig. 1.8a. At any time t > τ1 the area under the sc(t) sc(t1)

Dsc(t1)

sc(t0)

Dsc(t0) t1 t0 Time (a) Stress history consisting of two stress increments j(t,t)

J(t,t) j (t,t0)

J(t,t0) J(t,t1)

j(t,t1) t0

t1

(b) Creep coefficient

Time

t0

t1

Time

(c) Creep function

Figure 1.6 Creep coefﬁcients and creep functions associated with two stress increments.

12 Time-dependent deformation

ee(t)+ecr(t)

J(t,t0) Δsc(t0) + J(t,t1) Δsc(t1)

ecr(t)

j(t,t0) Δsc(t0)/Ec(t0)

J(t,t0) Δsc(t0)

t0

j(t,t0) Δsc(t0) /Ec(t0) + j(t,t1) Δsc(t1) /Ec(t1)

t1

t0

Time

(a) Elastic and creep deformations

t1

Time

(b) Creep deformation

Figure 1.7 Creep and elastic deformations due to two stress increments (Fig. 1.6a).

curve of Fig. 1.8b represents the actual stress-dependent deformation (sum of elastic and creep strains) at time t as deﬁned in Eq. 1.14. Consider the stress history shown in Fig. 1.9a. By dividing the time under load into n time steps, the continuously varying stress may be approximated by a series of small stress increments applied at the end of each time step. The stress-produced strains at time t are given by: εe (t) + εcr (t) =

n σc (τi ) i=0

Ec (τi )

[1 + ϕ(t, τi )] =

n

J(t, τi )σc (τi )

(1.15)

i=0

and a different creep coefﬁcient is required for each small stress increment, σ (τ i ). According to the principle of superposition, the total strain in concrete at time t subjected to the stress history shown in Fig. 1.9 is obtained by summing the stress-produced strains and the shrinkage strain: ε(t) = εe (t) + εcr (t) + εsh (t) ε(t) =

n

J(t, τi )σc (τi ) + εsh (t) =

i=0

n σc (τi ) i=0

Ec (τi )

+

n σc (τi )ϕ(t, τi ) i=0

J(t2,t)

J(t,t)

J(t2,t0)

J(t2,t1)

J(t2,t1)

J(t2,t0)

t0

t1 (a) Creep function

t2

Time

Ec (τi )

+ εsh (t) (1.16)

J(t2,t0) Ds(t0)

J(t2,t1) Ds (t1)

Ds(t0) Ds(t1) (b) Elastic plus creep deformations

Figure 1.8 Graphical representation of elastic plus creep deformation at time τ2 caused by two previous stress increments.

Time-dependent deformation 13 Creep function J(t,t0)

Stress

Hatched area = stress-produced strain (when stress increments are infinitesimally small)

Dsc(ti) sc(t)

i-th time interval Dti

Dsc(t0) t0 t1 t2

ti−1 ti Time

J(t,tn) sc(t0) Stress

t=tn

(a) Time-varying stress history

sc(tn)

(b) Stress-produced strains

Figure 1.9 Time-varying stress history and stress-produced strains.

In the limit, considering inﬁnitesimal stress increments dσ c (τ ), the summation included in Eq. 1.16 can be replaced by an integral: t

t J(t, τ )dσc (τ ) + εsh (t) =

ε(t) = τ0

τ0

1 + ϕ(t, τ ) dσc (τ ) + εsh (t) Ec (τ )

(1.17)

Equation 1.17 is referred to as the integral-type creep law (Ref. 12). The integral in Eq. 1.17 for the stress-produced strains is the area under the graph of creep function versus concrete stress in Fig. 1.9b. The stress at a point in a concrete structure under constant load often decreases with time as a result of creep. Consider the time-varying stress history shown in Fig. 1.10a where the initial stress σ c (τ 0 ) is compressive and decreases with time (i.e. all subsequent stress increments σ c (τ i ) are tensile). Notwithstanding the inaccuracies when the principle of superposition is applied to a decreasing stress history (mentioned previously), the stress produced strain may still be obtained using Eqs 1.16 or 1.17, with the integral in Eq. 1.17 represented by the hatched area under the curve in Fig. 1.10b. Creep function

Stress J(t,t0)

sc(t0) sc(t) Dsc(ti)

J(t,tn) i-th time interval t0 t1 t2

ti−1 ti Time

t = tn

(a) Gradually decreasing stress history

Hatched area = stress-produced strain (when stress increments are infinitesimally small) sc(tn) Stress

sc(t0)

(b) Stress-produced strain

Figure 1.10 Gradually decreasing stress history and stress-produced strain.

14 Time-dependent deformation The main disadvantage of the method of superposition, apart from its reduced accuracy when applied to a decreasing stress history, is the large amount of creep data required. Nevertheless, in a more general sense, the principle of superposition is relied upon in many ﬁelds of structural engineering and the analysis for time effects in concrete structures is no exception. 1.2.6 Tensile creep The previous discussions have been concerned with the creep of concrete in compression. However, the creep of concrete in tension is also of interest in a number of practical situations; for example, when studying the effects of restrained or differential shrinkage. Tensile creep also plays a signiﬁcant role in the analysis of suspended reinforced concrete slabs at service loads where stress levels are generally low and typically much of the slab is initially uncracked. Comparatively little attention has been devoted to the study of tensile creep (Ref. 1) and only limited experimental results are available in the literature, e.g. Ref. 13. Some researchers have multiplied the creep coefﬁcients measured for compressive stresses by factors in the range of 1 to 3 to produce equivalent coefﬁcient describing tensile creep (e.g. Refs 14 and 15). It appears that the mechanisms of creep in tension are different to those in compression. The magnitudes of both tensile and compressive creep increase when loaded at earlier ages. However, the rate of change of tensile creep with time does not decrease in the same manner as for compressive creep, with the development of tensile creep being more linear (Ref. 13). Drying tends to increase tensile creep in a similar manner to compressive creep and tensile creep is in part recoverable upon removal of the load. Further research is needed to provide clear design guidance. In this book, it is assumed that the magnitude and rate of development of tensile creep are similar to that of compressive creep at the same low stress levels. 1.2.7 The effects of creep on structural behaviour Creep is the time-dependent strain that develops in concrete due to sustained stress. When a loaded concrete member is unrestrained by steel reinforcement or by the external support conditions (such as a statically determinate plain concrete member), creep causes little more than an increase in deformations. The internal actions caused by imposed deformations in an indeterminate structure are proportional to stiffness. Due to creep, the internal actions caused by imposed deformations decrease with time in all concrete structures whether they are plain or reinforced. On the other hand, creep will not cause redistribution of loadinduced internal actions provided the creep characteristics are uniform throughout the structure. The effect of creep in this case is similar to a gradual and uniform change in the elastic modulus. Such a situation exists in an uncracked plain concrete member, if it is assumed that the creep characteristics of concrete in tension are the same as those in compression (which is a usual although not strictly correct assumption). The same is true in an uncracked reinforced concrete structure provided the reinforcement is symmetrical on each cross-section and uniform throughout the structure.

Time-dependent deformation 15 When portions of a statically indeterminate structure are made of different materials or of concrete with a different composition or age, and hence different creep characteristics, creep causes a redistribution of the load-induced internal actions. The internal actions are redistributed from the regions with the higher creep rate to the regions with the lower creep rate. In practical reinforced concrete ﬂexural members, the creep characteristics are rarely uniform throughout. Some regions are usually cracked and some are not. Reinforcement quantities usually vary along the length of the member and sections are seldom symmetrically reinforced. Nevertheless, the redistribution caused by creep of the load-induced bending moments and shear forces in statically indeterminate members is generally small and is quite often neglected in design. Creep can dramatically change the stress distribution on a reinforced concrete section. For example, stresses caused by shrinkage or temperature changes are relieved by creep. Creep also causes a redistribution of stresses between concrete and the bonded reinforcement on a cross-section. For example, consider a reinforced concrete column section subjected to a constant sustained axial compressive load. The concrete and steel are bonded together so that at any time compatibility requires that the concrete and steel strains are identical. As the compressive concrete creeps (contracts), the steel is compressed and the compressive stress in the steel gradually increases. Shrinkage causes a similar effect. Equilibrium requires that the increase in the compressive force in the steel is balanced by an equal and opposite tensile force on the concrete. Therefore, the compressive stress in the concrete reduces with time, while the steel stress increases rapidly. Load is thus transferred from the concrete to the steel, with the proportion of the external load carried by the reinforcement increasing with time. Fig. 1.11 shows the typical variation in compressive stresses in the concrete and steel caused by creep on the cross-section of an axially loaded reinforced concrete column subjected to a constant sustained compressive force, P. It is quite common, in fact, for the stress in the longitudinal reinforcement in typically proportioned reinforced concrete columns to be close to the yield stress at service loads, 300

sc = 10.0 MPa

10

ss = 242 MPa 250

Steel stress

Concrete stress 200 sc = 72.2 MPa

8 6

150

300 mm P = 1000 kN Ec = 25 GPa Es = 200 GPa j*(t) = 3.0

4

300 mm ss = 80.0 MPa

+

2

100

50

Steel compressive stress (MPa)

Concrete compressive stress (MPa)

12

As = 1500 mm2 0 0

t

Time (days)

0 10,000

Figure 1.11 Variation of stresses with time due to creep on a symmetrically reinforced axially loaded column section.

16 Time-dependent deformation due to the effects of creep and shrinkage (particularly for low-strength steel grades). The use of closely spaced lateral reinforcement in the form of closed ties or helices to prevent these highly stressed bars from buckling is therefore essential at the service load condition and not just at the ultimate load condition. The gradual development of creep strain on a reinforced concrete beam section causes an increase of curvature, as shown in Fig. 1.12, and a consequent increase in the beam deﬂection. For a plain concrete member, the increase in curvature is proportional to the creep coefﬁcient (i.e. the increase in curvature is proportional to the uniform increase in strain at every point on the section). For an uncracked, singly reinforced section (Fig. 1.12a), creep is restrained in the tensile zone by the reinforcement. Depending on the quantity of steel, the increase in curvature due to creep is proportional to a large fraction of the creep coefﬁcient (usually between 0.6ϕ(t) and 0.9ϕ(t)). On a cracked, singly reinforced beam section (Fig. 1.12b), the initial curvature is comparatively large and the cracked tensile concrete below the neutral axis can be assumed to carry no stress and therefore does not creep. Creep in the compression zone causes a lowering of the neutral axis and a consequent reduction in the compressive stress level. Creep is slowed down as the compressive stress reduces, and the increase in curvature is proportional to a small fraction of the creep coefﬁcient (usually less than one quarter). The relative increase in deﬂection caused by creep is therefore greater in an uncracked beam than in a cracked beam, although the total deﬂection in the cracked beam is signiﬁcantly greater. In prestressed concrete construction, in addition to causing increases in deﬂection (and camber), both creep and shrinkage cause shortening of the concrete member that in turn causes shortening of the prestressing tendons and a consequent reduction in the prestressing force. This loss of prestress may adversely affect the performance of the member at service loads and should be accounted for in its design. etop ≈etop(1+j) k0 k (t)

Ms

Time t Instantaneous

Section

Elevation

Strain

(a) Uncracked cross-section etop 0.7: Wire or strand: k5 = 5γ – 2.5 Alloy steel bars: k5 = (50γ – 29)/6

0 0.4 0.5 0.6 0.7 0.8 Stress in tendon as a proportion of fp, that is, g = sp,init /fp

Figure 2.4 Coefﬁcient, k5 (Ref. 2).

Creep in the prestressing steel may also be deﬁned in terms of a creep coefﬁcient ϕp (t, σp,init ) rather than as a relaxation loss. If the creep coefﬁcient for the prestressing steel ϕp (t, σp,init ) is the ratio of creep strain in the steel to the initial elastic strain, then the ﬁnal creep coefﬁcients for low relaxation wire, strand and bar are also given in Table 2.7 and may be approximated using Eq. 2.12. ϕp (t, σp,init ) =

R 1−R

(2.12)

Note that the creep of high-strength steels is non-linear with respect to stress. As has already been emphasised, creep (relaxation) of the prestressing steel depends on the stress level. In a prestressed concrete member, the stress in a tendon is gradually reduced with time as a result of creep and shrinkage in the concrete. This gradual reduction of stress results in a reduction of creep in the steel and hence smaller relaxation losses. To determine relaxation losses in a concrete structure therefore, the ﬁnal relaxation loss obtained from Eq. 2.11 (or Table 2.7) should be multiplied by a reduction factor, λr , that accounts for the time-dependent shortening of the concrete due to creep and shrinkage. The factor λr depends on the creep and shrinkage characteristics of the concrete, the initial prestressing force, and the stress in the concrete at the level of the steel, and can be determined by iteration (Ref. 17). However, because relaxation losses in modern prestressed concrete Table 2.7 Long-term relaxation losses and corresponding ﬁnal creep coefﬁcients for low relaxation wire, strand and bar (T = 20◦ C) Type of tendon

Wire Strand Bar

Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init ) Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init ) Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init )

Tendon stress as a proportion of fp 0.6

0.7

1.9 0.019 2.4 0.025 3.7 0.039

2.8 0.029 3.5 0.036 5.6 0.059

0.8 4.2 0.044 5.3 0.056 10.3 0.115

36 Material properties structures (employing low-relaxation steels) are relatively small, it is usually sufﬁcient to take λr ≈ 0.8. When elevated temperatures exist during curing (i.e. steam curing), relaxation is increased and occurs rapidly during the curing cycle. For low relaxation steel in a concrete member subjected to an initial period of steam curing, it is recommended that the design relaxation be taken signiﬁcantly greater than the value given by Eq. 2.11 (calculated with T = 20◦ C).

2.3 References 1. Gilbert, R.I. (2002). Creep and shrinkage models for high strength concrete – proposals for inclusion in AS3600. Australian Journal of Structural Engineering, IEAust, 4(2), 95–106. 2. Standards Australia (2009). Australian Standard for Concrete Structures, AS3600–2009. Sydney. 3. ACI Committee 209 (2008). Guide for modeling and calculating shrinkage and creep in hardened concrete (ACI 209.2R-8). American Concrete Institute, Farmington Hills, Michigan. 4. ACI Committee 209 (1992). Prediction of creep, shrinkage, and temperature effects in concrete structures (ACI 209R-92). American Concrete Institute, Farmington Hills, Michigan. 5. Bazant, Z.P. and Baweja, S. (2000). Creep and shrinkage prediction model for analysis and design of concrete structures: model B3. The Adam Neville Symposium: Creep and Shrinkage – Structural Design Effects, ACI SP-194. American Concrete Institute, Farmington Hills, Michigan, 236–260. 6. Bazant, Z.P. and Baweja, S. (1995). Creep and shrinkage prediction model for analysis and design of concrete structures – model B3. Materials and Structures, 28, 357–365. 7. Comité Euro-International du Béton (1993). CEB-FIB Model Code 1990: Design Code. Thomas Telford, London. 8. Comité Euro-International du Béton (1999). Structural concrete – Textbook on behaviour, design and performance – Volume 2: Basis of design. Fib Bulletin No. 2, Federation Internationale du Béton, Lausanne, Switzerland, 37–52. 9. British Standard (2004). BS EN 1992, Eurocode 2: Design of concrete structures - Part 1-1: general rules and rules for buildings. British Standards Institute, Milton Keynes. 10. Gardner, J. and Lockman, M.J. (2001). Design provisions for drying shrinkage and creep of normal-strength concrete. ACI Materials Journal, 98(2), 159–167. 11. Comité Euro-International du Béton (1984). CEB Design manual on structural effects of time-dependent behaviour of concrete. M.A. Chiorino (ed.), Georgi Publishing, SaintSaphorin, Switzerland. 12. Pauw, A. (1960). Static Modulus of Elasticity of Concrete as Affected by Density. ACI Journal, 57(6), 679–687. 13. Gilbert, R.I. (1988). Time Effects in Concrete Structures. Elsevier Science Publishers, Amsterdam. 14. Bazant, Z.P. and Li, G.-H. (2008). Unbiased statistical comparison of creep and shrinkage prediction models. ACI Materials Journal, 105(6), 610–619. 15. Chiorino, M.A. (2005). A rational approach to the analysis of creep structural effects. Shrinkage and Creep of Concrete, SP-227, American Concrete Institute, Farmington Hills, Michigan, 107–141. 16. Brooks, J.J. (2005). 30-year creep and shrinkage of concrete. Magazine of Concrete Research, 57(9), 545–556. 17. Ghali, A., Favre, R., and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London.

3

Design for serviceability Deﬂection and crack control

3.1 Introduction The tensile capacity of concrete is usually neglected when calculating the strength of a reinforced concrete member, even though the concrete continues to carry tensile stress between the cracks due to the transfer of forces from the tensile reinforcement to the concrete through bond. This contribution of the tensile concrete is known as tension stiffening and it affects the stiffness of the member after cracking and hence its deﬂection and the width of the cracks. Reinforced concrete members often contain relatively small quantities of tensile reinforcement, in some situations close to the minimum amount permitted by the relevant building code. This is particularly so in the case of ﬂoor slabs. For such members, the ﬂexural rigidity of a fully cracked cross-section (Ec Icr ) is many times smaller than that of an uncracked cross-section (Ec Iuncr ) and tension stiffening contributes greatly to the member’s stiffness after cracking. In structural design, deﬂection and crack control at service load levels are usually the governing considerations and accurate modelling of the stiffness after cracking is required. In-service deﬂections depend primarily on the properties of the concrete and these are often not known reliably at the design stage. The non-linear behaviour that complicates serviceability calculations is due to cracking, tension stiffening, creep and shrinkage of the concrete. Of these, shrinkage is perhaps the most problematic. Shrinkage may cause time-dependent cracking that reduces member stiffness and gradually reduces the beneﬁcial effects of tension stiffening. It results in a gradual widening of existing cracks and, in ﬂexural members, a signiﬁcant increase in deﬂections with time. The problem is particularly difﬁcult in the case of slabs that are typically shallow, with relatively large span to depth ratios, and are therefore deﬂection sensitive. The ﬁnal deﬂection of a slab depends very much on the extent of initial cracking which, in turn, depends on the construction procedure (shoring and re-shoring), the amount of early shrinkage, the temperature gradients in the ﬁrst few weeks after casting, the degree of curing and so on. Many of these parameters are, to a large extent, outside of the control of the designer. In ﬁeld measurements of the deﬂection of many identical slab panels (Refs 1 and 2), large variability was reported. Deﬂections of identical panels after one year differed by over 100 per cent in some cases. These differences can be attributed to the different conditions (both in terms of load and environment) that existed in the ﬁrst few weeks after the casting of each slab.

38 Design for serviceability Serviceability failures of concrete structures involving excessive cracking and/or excessive deﬂection are relatively common. Numerous cases have been reported of structures that complied with the local code requirements but still deﬂected or cracked excessively (Refs 1–3). In many of these cases, shrinkage of the concrete was primarily responsible or, probably more precisely, failure to adequately account for shrinkage (and creep) in the design was primarily responsible. The need for a more reliable deﬂection calculation procedure has been exacerbated by the introduction, in recent years, of higher strength reinforcing steels. The use of higher strength steel usually means that less steel is required for strength and, consequently, less stiffness is available after cracking, leading to greater deﬂection and wider cracks under service loads. Design for serviceability has increasingly assumed a more prominent role in the design of both beams and slabs. This chapter describes the behaviour of reinforced concrete elements under service loads and outlines the simpliﬁed approaches for deﬂection and crack control that are speciﬁed in modern design codes, including ACI 318-08 (Ref. 4), Eurocode 2 (Refs 5 and 6) and AS 3600-2009 (Ref. 7). The limitations of these simpliﬁed approaches are discussed and the need for the more reﬁned methods of analysis at the serviceability limit states that are described in subsequent chapters is demonstrated.

3.2 Design objectives and criteria The broad design objective for a concrete structure is that it should satisfy the needs for which it was contrived. In doing so, the structural designer must ensure that it is safe and serviceable, so that the chance of it failing during its design lifetime is sufﬁciently small. Structural failure can take a variety of forms. The structure must be strong enough and sufﬁciently ductile to resist, without collapse, the overloads and environmental extremes that may be imposed upon it. It must also perform satisfactorily under day-to-day service loads without deforming, cracking or vibrating excessively. The two primary structural design objectives are therefore strength and serviceability. Other structural design objectives are stability and durability – a structure must be stable and resist overturning or sliding; reinforcement must not corrode; concrete must resist abrasion and spalling, and the structure must not suffer a signiﬁcant reduction of strength or serviceability with time. Another non-structural, but important, objective is aesthetics and, of course, an overarching design objective is economy. Ideally, the structure should be in harmony with, and enhance, the environment and this often requires collaboration between the structural engineer, environmental engineer and architect. The aim is to achieve, at minimum cost, an aesthetically pleasing and functional structure that satisﬁes the required structural objectives. In order for design calculations to proceed for a particular structure, the design objectives must be translated into quantitative terms called design criteria. For example, the designer needs to determine the maximum acceptable deﬂection for a particular beam or slab, or the maximum crack width that can be tolerated in a concrete ﬂoor or wall. Also required are minimum numerical values for the strength of individual elements or connections. It is also necessary to identify and quantify all of the loads or actions that will be applied to the structure and the probability of their occurrence. The design criteria are speciﬁed in codes of practice and provide a suitable margin of safety (called the safety index) against a structure becoming unﬁt for service in any way.

Design for serviceability

39

The speciﬁc form of the design criteria depends on the philosophy and method of design adopted by the relevant code and the manner in which the inherent variability in both the load and the structural performance is considered. Modern design codes for structures have generally adopted the limit states method of design, whereby a structure must be designed to simultaneously satisfy a number of different limit states or design requirements, including adequate strength and serviceability. Minimum performance criteria are speciﬁed for each of these limit states and any one may become critical and govern the design of a particular member. If a structure ceases to fulﬁl its intended function in any way, it is said to enter a limit state. Each possible mode of failure is a limit state. For each limit state, codes of practice specify both load combinations and methods of predicting the actual structural performance that together ensure an acceptably low probability of failure, depending on the consequences and cost of the failure. For the strength limit states, the consequences of failure are high and so the probability of failure must be very low. For the serviceability limit states, such as excessive deﬂection or excessive cracking, the consequences of failure are not as great and a higher probability of failure is justiﬁable. Design for the serviceability limit states involves making reliable predictions of the time-dependent deformation of the concrete structure. This is complicated by the nonlinear material behaviour of concrete, caused mainly by cracking, tension stiffening, creep and shrinkage. This book deals primarily with the inclusion of these material non-linearities in the analysis of concrete structures, and so it is primarily concerned with designing for serviceability. In order to satisfy the serviceability limit states, a concrete structure must be serviceable and perform its intended function throughout its working life. Excessive deﬂection should not impair the function of the structure or be aesthetically unacceptable. Excessive deﬂection should also not cause unintended load paths, such as occurs when a deﬂecting slab begins to bear on a non-load-bearing partition. Cracks should not be unsightly or wide enough to lead to durability problems and vibration should not cause distress to the structure or discomfort to its occupants.

3.3 Design actions In the design of concrete structures for the serviceability limit states, the internal actions and deformations that arise from appropriate combinations of the day-to-day service loads should be considered, including, where applicable: dead load (G); live load (Q); wind load (W); prestress (P); earthquake load (Feq ); earth pressure (Fep ); liquid pressure (Flp ); and snow load (Fs ). In addition, any accidental loading and loads arising during construction should be considered where they may adversely affect the various limit states’ requirements. Other actions that may affect the serviceability of the structure include, creep of concrete, shrinkage of concrete and other imposed deformations, such as may result from temperature changes and gradients, support settlements and foundation movements. Dead loads are generally deﬁned as those loads imposed by both the structural and non-structural components of a structure. Dead loads include the self-weight of the structure and the forces imposed by all walls, ﬂoors, roofs, ceilings, permanent partitions, service machinery and other permanent construction. Dead loads are usually permanent, ﬁxed in position and can be estimated reasonably accurately from the mass of the relevant material or type of construction. For example, normal weight

40 Design for serviceability concrete weighs about 24 kN/m3 . Lightweight reinforced concrete weighs between 15 and 20 kN/m3 . Live loads are the loads that are attributed to the intended use or purpose of the structure and are generally speciﬁed by regional or national codes and speciﬁcations, such as Refs 8–13. The speciﬁed live load depends on the expected use or occupancy of the structure and usually includes allowances for impact and inertia loads (where applicable) and for possible overload. Both uniformly distributed and concentrated live loads are normally speciﬁed. The magnitude and distribution of the actual live load is never known accurately at the design stage, and it is by no means certain that the speciﬁed live load will not be exceeded at some stage during the life of the structure. Live loads may or may not be present at any particular time; they are not constant and their position can vary. Although part of the live load is transient, some portion may be permanently applied to the structure and have effects similar to dead loads. Live loads also arise during construction due to the stacking of building materials, the use of particular equipment or the construction procedure (such as the loads induced by ﬂoor-to-ﬂoor propping in multi-storey construction). The speciﬁed wind, earthquake, snow and temperature loads depend on the geographical location and relative importance of the structure (the mean return period). Wind loads also depend on the surrounding terrain and the height of the structure above the ground. These environmental loads are also usually speciﬁed by regional or national codes and speciﬁcations, such as Refs 13–16. The design loads to be used in serviceability calculations are the day-to-day service loads and these may be considerably less than the speciﬁed loads. For example, the speciﬁed live load, Q, has a built-in allowance for overload and impact. There is a low probability that it will be exceeded. It is usually not necessary, therefore, to ensure acceptable deﬂections and crack widths under the full speciﬁed loads. Use of the actual load combinations under normal conditions of service – the expected loads – is more appropriate. Often, codes of practice differentiate between the speciﬁed (or characteristic) loads and the expected loads. Depending on the type of structure, the expected loads may be signiﬁcantly less than the speciﬁed loads. If the aim of the serviceability calculation is to produce a best estimate of the likely behaviour, then expected loads should be considered. Often the magnitudes of the expected loads are not deﬁned and are deemed to be a matter of engineering judgment. In some codes, serviceability load factors (ψ ≤ 1.0) are nominated to determine the expected load from the speciﬁed load for both short-term (ψ1 Q) and long-term loading (ψ2 Q). If the aim is to satisfy a particular serviceability limit state and the consequences of failure to do so are high, then the speciﬁed loads may be more appropriate. Once again, the decision should be based on engineering judgment and experience. With regard to dead loads, the expected and speciﬁed values are the same and therefore the speciﬁed dead load should be used in all serviceability calculations. For live loads, the expected values should be used when a best estimate is required. For building structures, the expected live load for short-term serviceability load combinations is usually about 70 per cent of the speciﬁed live load for dwellings (i.e. ψ1 = 0.7), 60 per cent for retail areas, 50 per cent for ofﬁces and parking areas and 100 per cent for storage areas. For bridges, the live load for short-term serviceability load combinations is usually taken to be about 70 per cent of the speciﬁed live load for spans of less than about 10 m, reducing to 50 per cent for spans greater than 100 m.

Design for serviceability

41

For long-term serviceability calculations, the following percentages of the speciﬁed live load are usually considered as permanent or sustained (with the remainder being transitory in nature): 30 per cent for dwellings and retail stores (i.e. ψ2 = 0.3), 25 per cent for parking areas, 20 per cent for ofﬁces, and 50–80 per cent for storage areas. With the appropriate design actions for serviceability determined, the response of the structure must satisfy the relevant design criteria for deﬂection and crack control. These are usually also embodied in the codes of practice and are discussed in the following sections.

3.4 Design criteria for serviceability 3.4.1 Deﬂection limits The design for serviceability, particularly the control of deﬂections, is frequently the primary consideration when determining the cross-sectional dimensions of beams and ﬂoor slabs in concrete buildings. This is particularly so in the case of slabs, as they are typically thin in relation to their spans and are therefore deﬂection sensitive. It is stiffness rather than strength that usually controls the design of slabs, particularly in the cases of ﬂat slabs and ﬂat plates. Most concrete design codes, including ACI 318-08 (Ref. 4), Eurocode 2 (Ref. 6) and the Australian Standard AS 3600-2009 (Ref. 7), specify two basic approaches for deﬂection control. The ﬁrst and simplest approach is deﬂection control by the satisfaction of a minimum depth requirement or a maximum span-to-depth ratio (see Section 3.5). The second approach is deﬂection control by the calculation of deﬂection, where the deﬂection (or camber) is calculated using realistic models of material and structural behaviour. This calculated deﬂection should not exceed the deﬂection limits that are appropriate to the structure and its intended use. The deﬂection limits should be selected by the designer and are often a matter of engineering judgment. Codes of practice give general guidance for both the selection of the maximum deﬂection limits and the calculation of deﬂection. However, the simpliﬁed procedures for calculating the deﬂections of beams and slabs in most codes are necessarily design-oriented and simple to use, involving crude approximations of the complex effects of cracking, tension stiffening, concrete creep, concrete shrinkage and the load history (see Section 3.6). Generally, they have been developed and calibrated for simply-supported reinforced concrete beams (Ref. 17) and often produce inaccurate and non-conservative predictions when applied to lightly reinforced concrete slabs (Ref. 18). In addition, most existing code procedures do not provide real guidance on how to adequately model the time-dependent effects of creep and shrinkage in deﬂection calculations. There are three main types of deﬂection problem that may affect the serviceability of a concrete structure: 1 2 3

where excessive deﬂection causes either aesthetic or functional problems; where excessive deﬂection results in unintended load paths or damage to either structural or non-structural elements attached to the member; where dynamic effects due to insufﬁcient stiffness cause discomfort to occupants.

42 Design for serviceability Examples of deﬂection problems of type 1 include visually unacceptable sagging (or hogging) of slabs and beams and ponding of water on roofs. Type 1 problems are generally overcome by limiting the magnitude of the ﬁnal long-term deﬂection (here called total deﬂection) to some appropriately low value. The total deﬂection of a beam or slab in a building is usually the sum of the short-term and time-dependent deﬂections caused by the dead load (including self-weight), the prestress (if any), the expected in-service live load and the load-independent effects of shrinkage and temperature change. When the total deﬂection exceeds about span/200 below the horizontal, it may become visually unacceptable. Total deﬂection limits that are appropriate for the particular member and its intended function must be selected by the designer. For example, a total deﬂection limit of span/200 may be appropriate for the ﬂoor of a car park, but would be totally inadequate for a gymnasium ﬂoor that is required to remain essentially plane under service conditions and where functional problems arise at very small total deﬂections. AS 3600-2009 (Ref. 7) requires that a limit on the total deﬂection be selected that is appropriate to the structure and its intended use, but that limit should not be greater than span/250 for a span supported at both ends and span/125 for a cantilever (see Table 3.1). Examples of type 2 problems include deﬂection-induced damage to ceiling or ﬂoor ﬁnishes, cracking of masonry walls and other brittle partitions, improper functioning of sliding windows and doors, tilting of storage racking and so on. To avoid these problems, a limit must be placed on that part of the total deﬂection that occurs after the attachment of the non-structural elements in question, that is, the incremental deﬂection. This incremental deﬂection is the sum of the long-term deﬂection due to all of the sustained loads and shrinkage, the short-term deﬂection due to the transitory live load and the short-term deﬂection due to any dead load applied to the structure after the attachment of the non-structural elements under consideration, together with any temperature-induced deﬂection. For roof or ﬂoor construction supporting or attached to non-structural elements that are likely to be damaged by large deﬂection, ACI 318-08 (Ref. 4) limits the incremental deﬂection to span/480 (and span/240 when the non-structural elements are unlikely to be damaged by deﬂection). Incremental deﬂections of span/480 can, in fact, cause cracking in supported masonry walls, particularly when doorways or corners prevent arching and when no provisions are made to minimise the effect of movement. AS 3600-2009 limits the incremental deﬂection for members supporting masonry partitions or other brittle ﬁnishes to between span/500 and span/1000 depending on the provisions made to minimise the effect of movement (see Table 3.1). Eurocode 2 (Ref. 6) recommends limits on total (incremental) deﬂection of span/250 (span/500). Type 3 deﬂection problems include the perceptible springy vertical motion of ﬂoor systems and other vibration-related problems. Very little quantitative information for controlling this type of deﬂection problem is available in codes of practice. For a ﬂoor that is not supporting or attached to non-structural elements likely to be damaged by large deﬂection, ACI 318-08 (Ref. 4) places a limit of span/360 on the short-term deﬂection due to live load (and span/180 for a ﬂat roof). This limit provides a minimum requirement on the stiffness of members that may, in some cases, be sufﬁcient to avoid type 3 problems. Such problems are potentially the most common for prestressed concrete ﬂoors, where load balancing is often employed to produce a nearly horizontal ﬂoor under the sustained load and the bulk of the ﬁnal deﬂection is due to the transient

Design for serviceability

43

Table 3.1 Limits for calculated deﬂections of beams and slabs with effective span ef Type of member

Deﬂection to be considered

Deﬂection limitation for spans (Notes 2 and 3)

Deﬂection limitation for cantilevers (Note 5)

All members Members supporting masonry partitions

The total deﬂection The deﬂection that occurs after the addition or attachment of the partitions

ef /250 ef /500 where provision is made to minimise the effect of movement, otherwise ef /1000

Members supporting other brittle ﬁnishes

The deﬂection that occurs after the addition or attachment of the ﬁnish The imposed action (live load and dynamic impact) deﬂection Total deﬂection

Manufacturer’s speciﬁcation but not more than ef /500

ef /125 ef /250 where provision is made to minimise the effect of movement, otherwise ef /500 Manufacturer’s speciﬁcation but not more than ef /250

ef /800

ef /400

ef /500 where provision is made to minimize the effect of deﬂection of the transfer member on the supported structure, otherwise ef /1000

ef /250

Members subjected to vehicular or pedestrian trafﬁc Transfer members

1 2 3 4 5 6 7

The effective span ef is the lesser of the centre-to-centre distance between the supports and the clear span plus the member depth. For a cantilever ef is the clear projection plus half the member depth. In general, deﬂection limits should be applied to all spanning directions. This includes, but is not limited to, each individual member and the diagonal spans across each design panel. For ﬂat slabs with uniform loadings, only the column strip deﬂections in each direction need be checked. If the location of masonry partitions or other brittle ﬁnishes is known and ﬁxed, these deﬂection limits need only be applied to the length of the member supporting them. Otherwise, the more general requirements of Note 2 should be followed. Deﬂection limits given may not safeguard against ponding. For cantilevers, the deﬂection limitations given in this table apply only if the rotation at the support is included in the calculation of deﬂection. Consideration should be given by the designer to the cumulative effect of deﬂections, and this should be taken into account when selecting a deﬂection limit. When checking the deﬂections of transfer members and structures, allowance should be made in the design of the supported members and structure for the deﬂection of the supporting members. This will normally involve allowance for settling supports and may require continuous bottom reinforcement at settling columns.

live load. Such structures are generally uncracked at service loads, the total deﬂection is small and type 1 and 2 deﬂection problems are easily avoided. Where a structure supports vibrating machinery (or any other signiﬁcant dynamic load) or where a structure may be subjected to ground motion caused by earthquake, blast or adjacent road or rail trafﬁc, vibration control becomes an important design requirement. This is particularly so for slender structures, such as tall buildings or long-span beams or slabs.

44 Design for serviceability Vibration is best controlled by isolating the structure from the source of vibration. Where this is not possible, vibration may be controlled by limiting the frequency of the fundamental mode of vibration of the structure to a value that is signiﬁcantly different from the frequency of the source of vibration. When a structure is subjected only to pedestrian trafﬁc, 5 Hz is often taken as the minimum frequency of the fundamental mode of vibration of a beam or slab (Refs 19 and 20) and a method for vibration analysis is described in Ref. 20. In modern concrete structures, serviceability failures are relatively common. The tendency towards higher strength materials and the use of ultimate strength design procedures for the proportioning of structures has led to shallower, more slender elements, and consequently, an increase in deformations at service loads. As far back as 1967 (Ref. 21), the most common cause of damage in concrete structures was due to excessive slab deﬂections. If the incidence of serviceability failure is to decrease, design for serviceability must play a more signiﬁcant part in routine structural design and the structural designer must resort more often to analytical tools that are more accurate than those found in most building codes. The analytical models outlined in the remainder of this book provide designers with reliable and rational means for predicting both the short-term and time-dependent deformations in concrete structures. 3.4.2 Crack width limits In routine structural design, the calculation of crack widths is often not required. Crack control is deemed to be provided by appropriate detailing of the reinforcement and by limiting the stress in the reinforcement crossing the crack to some appropriately low value (see Section 3.7.1). The limiting steel stress depends on the maximum acceptable crack width for the structure that in turn depends on the structural requirements and the local environment. Recommended maximum crack widths are given in Table 3.2.

3.5 Maximum span-to-depth ratio – minimum thickness In the design of a reinforced concrete beam or slab, the designer is ﬁrst confronted with the problem of selecting a suitable depth or thickness of the member. In the case of ﬂoor slabs, a reasonable ﬁrst estimate is desirable since, in many cases, the self-weight of the slab is a large proportion of the total service load. Strength considerations alone may result in a slab thickness that leads to excessive deﬂection at service loads. The relatively low tensile reinforcement quantities commonly used in slabs (Ast /bd is typically in the range 0.0025–0.006) are evidence of the importance of serviceability in the selection of slab thickness. Many codes of practice specify a minimum thickness, h, or a maximum span-toeffective depth ratio, /d. The implication is that deﬂection will be acceptable if the beam or slab thickness is greater than the minimum value, and thus the deﬂection need not be calculated. For example, for normal weight concrete members containing steel reinforcement with a yield stress of fy = 500 MPa and for members that are not supporting or attached to partitions or other construction likely to be damaged by large deﬂection, ACI-318-08 (Ref. 4) speciﬁes that deﬂections need not be calculated if the thickness of a beam or one-way slab is greater than the minimum thickness given in Table 3.3

Design for serviceability

45

Table 3.2 Recommended maximum ﬁnal design crack width, w∗ Environment

Design requirement

Sheltered environment (where crack widths will not adversely affect durability)

Aesthetic requirement • where cracking could adversely affect the appearance of the structure • close in buildings • distant in buildings

0.3 0.5

•

0.7

Environment

Aggressive environment ∗c

Maximum ﬁnal crack width, w* (mm)

where cracking will not be visible and aesthetics is not important.

Durability requirement • where wide cracks could lead to corrosion of reinforcement

0.3

Durability requirement • where wide cracks could lead to corrosion of reinforcement

0.30 (when c∗ ≥ 50 mm) 0.25 (otherwise)

is the concrete cover to the nearest steel reinforcement.

Table 3.3 Minimum thickness for non-prestressed beams or one-way slabs – fy = 500 MPa (Ref. 4) Minimum thickness, h

Solid one-way slab Beam or ribbed slab

Simplysupported

One end continuous

Both ends continuous

Cantilever

/18 /14.5

/21.5 /16.5

/25 /19

/9 /7

is the span measured centre to centre of supports or the clear projection of a cantilever.

or if the thickness of a two-way ﬂat slab or ﬂat plate is greater than the value given in Table 3.4. This deemed-to-comply approach is attractive because of its simplicity and, if it always led to appropriately proportioned and serviceable slabs, it would be ideal for use in routine design. However, in some situations, the use of the minimum thicknesses in Tables 3.3 and 3.4 leads to slabs that are far thicker than they need to be. In other situations, some heavily loaded slabs with the minimum thicknesses speciﬁed in Tables 3.3 and 3.4 deﬂect excessively. Indeed, a single value for minimum thickness that does not account for the load level, the steel quantities and location, the occupancy of the structure (and therefore the desired deﬂection limit), the load duration, the quality of the concrete and the environment cannot possibly ensure deﬂection control in every situation, unless, of course, it is grossly conservative in many situations and therefore entirely unsuitable for use in structural design. Based on the work of Rangan (Ref. 22) and Gilbert (Ref. 23), the Australian Standard AS3600-2009 (Ref. 7) speciﬁes a maximum span to effective depth ratio

46 Design for serviceability Table 3.4 Minimum thickness of two-way slabs without interior beams (ﬂat slabs or ﬂat plates) – fy = 500 MPa (Ref. 4) Minimum thickness, h Without drop panels

With drop panels

Exterior panels Without edge beams n /28

Interior panels With edge beams n /31

n /31

Exterior panels Without edge beams n /31

Interior panels With edge beams n /34

n /34

n is the clear span measured face to face of supports in long span direction.

for slabs given by: ef /d = k3 k4

(/ef )1000Ec

1/3

Fd.ef

(3.1)

where ef is the lesser of the clear span plus slab thickness and the centre-to-centre distance between supports; d is the effective depth from the compressive surface of the slab to the centroid of the tensile reinforcement; is the deﬂection limit selected in design (either total or incremental deﬂection); Ec is the elastic modulus of the concrete (in MPa); Fd.ef is the effective design service load (in kPa) and is equal to 3g + q1 + 2q2 for total deﬂection and 2g + q1 + 2q2 for incremental deﬂection; g is the dead load (in kPa); q1 is the expected short-term live load (in kPa); q2 is the sustained part of the live load (in kPa); and k3 is a slab system factor given by: • • •

k3 = 1.0 for one-way slabs and two-way edge-supported slabs; k3 = 0.95 for a two-way ﬂat slab without drop panels; and k3 = 1.05 for a two-way ﬂat slab with drop panels.

The term k4 is a factor that depends on the continuity at the supports of the slab and, for a one-way slab or two-way ﬂat slab, k4 equals 1.4 for a simply-supported span, l.75 for the end span of a continuous slab and 2.1 for an interior span of a continuous slab. For a two-way edge-supported slab, k4 is given in Table 3.5. Alternative expressions for the limiting span-to-depth ratios are speciﬁed in other codes. For example, according to Eurocode 2 (Ref. 6), if the span-to-depth ratio of a member does not exceed the following limiting values, deﬂections need not be calculated for members where the maximum total deﬂection is not to exceed span/250 and where the incremental deﬂection is not to exceed span/500:

3/2 ρo ρo if ρ ≤ ρo −1 = K 11 + 1.5 fc + 3.2 fc ρ ρ d ρ 1 ρ o + f if ρ > ρo = K 11 + 1.5 fc c d ρ − ρ 12 ρo

(3.2a)

(3.2b)

Design for serviceability

47

Table 3.5 Continuity factor k4 for a rectangular slab panel supported on four sides – (Ref. 7) Edge condition

Continuity factor, k4 Ratio of long to short span (y /x )

Four edges continuous One short edge discontinuous One long edge discontinuous Two short edges discontinuous Two long edges discontinuous Two adjacent edges discontinuous Three edges discontinuous (one long edge continuous) Three edges discontinuous (one short edge continuous) Four edges discontinuous

1.0

1.25

1.5

2.0

3.60 3.40 3.40 3.20 3.20 2.95 2.70 2.70 2.25

3.10 2.90 2.65 2.80 2.50 2.50 2.30 2.10 1.90

2.80 2.70 2.40 2.60 2.00 2.25 2.20 1.90 1.70

2.50 2.40 2.10 2.40 1.60 2.00 1.95 1.60 1.50

where K depends on the structural system, with K = 1.0 for simply supported beams and one-way or two-way spanning slabs; K = 1.3 for end spans of continuous beams and one-way or two-way slabs continuous over one long side; K = 1.5 for interior spans of beams and one-way or two-way spanning slabs; K = 1.2 for ﬂat slabs supported on columns without beams (based on longer span); and K = 0.4 for a cantilever; ρo is a reference reinforcement ratio given by ρo = 0.001 fc ; ρ is the tension reinforcement ratio at mid-span required to resist the moment due to the design loads (at the support for cantilevers); ρ is the compression reinforcement ratio at mid-span (at the support for cantilevers); fc is in MPa. For ﬂanged sections where the ratio of the ﬂange width to the web width exceeds 3, the values obtained from Eqs 3.2 should be multiplied by 0.8. For beams and slabs, other than ﬂat slabs, supporting partitions likely to be damaged by excessive deﬂection and with spans exceeding 7 m, the values of /d given by Eqs 3.2 should be multiplied by 7/ef , where ef is the effective span in metres. For ﬂat slabs supporting partitions likely to be damaged by excessive deﬂection and where the longer span exceeds 8.5 m, the values of /d given by Eqs 3.2 should be multiplied by 8.5/ef . An iterative procedure is required to use Eqs 3.2. An initial estimate of the effective depth d must be made in order to calculate the reinforcement ratios ρ and ρ required to resist the design moment at the critical sections. These reinforcement ratios are in turn required in the calculation of the limiting span-to-depth ratio using Eqs 3.2. Depending on the initial estimate of d, the required reinforcement ratios may need to be recalculated, together with a revised slab depth, to ensure deﬂection control. Similarly, the use of Eq. 3.1 requires an initial estimate of slab thickness to determine the self-weight and an iteration may be required if the initial estimate is poor. On the other hand, the ACI 318-08 (Ref. 4) minimum thicknesses do not require any iteration and can be used to select an initial member thickness at the beginning of the design. Designers should be aware that the use of either the ACI 318-08 minimum thicknesses (Tables 3.3 and 3.4) or the AS3600-2009 (Ref. 7) maximum span-todepth ratio (Eq. 3.1) is inevitably conservative for most practical situations and leads

48 Design for serviceability to beam and slab thicknesses that may be considerably larger than they need to be. In contrast, the Eurocode 2 (Ref. 6) limiting span-to-depth ratios may result in beam or slab thicknesses that are unacceptably small, particularly in situations where the sustained load is a large proportion of the total load, and should not be regarded as a guarantee that deﬂections will not be excessive.

Example 3.1 The thickness of the end span of a one-way slab is to be estimated for the cases where: 1) the maximum long-term mid-span deﬂection is not to exceed span/250; and 2) the incremental deﬂection is not to exceed span/480. The span is = ef = 5.0 m; the dead load g = 2.0 kPa + self-weight; and the live load is q = 3.0 kPa. The short-term expected live load is q1 = 2.1 kPa and the sustained part of the live load q2 = 1.2 kPa. The speciﬁed concrete and reinforcement strengths are fc = 25 MPa and fy = 500 MPa; the clear concrete cover to the longitudinal reinforcement is 20 mm; and the reinforcement bar diameter is db = 12 mm.

ACI318-08 From Table 3.3, if deﬂections are not to be calculated, the minimum thickness according to ACI318-08 is h = 5000/21.5 = 230 mm, irrespective of the deﬂection requirements for the slab and irrespective of the loads to be applied to the slab.

AS3600-2009 From Table 2.1, Ec = 26700 MPa. To calculate the maximum effective span-todepth ratio using Eq. 3.1, an estimate of self-weight of the slab is required. Take self-weight = 0.23 × 24 = 5.5 kPa and the dead load is therefore g = 2.0 + 5.5 = 7.5 kPa. (i) If the maximum total deﬂection is = 5000/250 = 20 mm, then the effective design service load is Fd.ef = 3g + q1 + 2q2 = 3 × 7.5 + 2.1 + 2 × 1.2 = 27.0 kPa and, from Eq. 3.1, the maximum span to effective depth ratio is:

ef /d = 1.0 × 1.75

(20/5000) × 1000 × 26700 27.0

1/3 = 27.7

The minimum effective depth according to AS 3600-2009 is therefore d = 5000/27.7 = 181 mm and the minimum slab thickness is h = d + db /2 + cover = 181 + 6 + 20 = 207 mm.

Design for serviceability

49

(ii) If the incremental deﬂection is = 5000/480 = 10.4 mm, then the effective design service load is Fd.ef = 2g + q1 + 2q2 = 2 × 7.5 + 2.1 + 2 × 1.2 = 19.5 kPa and, from Eq. 3.1, the maximum span to effective depth ratio is:

ef /d = 1.0 × 1.75

(10.4/5000) × 1000 × 26700 19.5

1/3 = 24.8

The minimum effective depth according to AS 3600-2009 is therefore d = 5000/24.8 = 201 mm and the minimum slab thickness is h = d + db /2 + cover = 201 + 6 + 20 = 227 mm.

Eurocode 2 If the design moment at mid-span is w∗ 2 /12, where w∗ is the factored design load for the strength limit state, and if after several iterations the initial estimate of d is 150 mm, the reinforcement ratio required to resist the design moment is ρ = 0.0035 and ρ = 0. The reference reinforcement ratio is ρo = 0.001 fc = 0.005 and the factor K = 1.3. From Eq. 3.2a:

3/2 √ √ 0.005 0.005 = 1.3 11 + 1.5 25 = 34.1 + 3.2 25 −1 d 0.0035 0.0035 The minimum effective depth according to Eurocode 2 is therefore d = 5000/34.1 = 147 mm and the minimum slab thickness is h = d + db /2 + cover = 147 + 6 + 20 = 173 mm. Clearly, in this example, the minimum slab thickness obtained using Eq. 3.2a from Eurocode 2 is signiﬁcantly smaller than the value obtained using either the ACI 318-08 minimum thickness provisions or the maximum span to depth ratio speciﬁed in AS 3600-2009.

3.6 Deﬂection control by simpliﬁed calculation 3.6.1 Calculation of deformation If the axial strain and curvature are known at regular intervals along a member, it is a relatively simple task to determine the deformation of that member. Consider the statically determinate member subjected to the axial and transverse loads shown in Fig. 3.1. The axial deformation of the member eAB (either elongation or shortening) is obtained by integrating the axial strain at the centroid of the member, εa (z), over the length of the member. That is: eAB =

0

εa (z) dz

where z is measured along the member, as shown.

(3.3)

50 Design for serviceability Load B

A C /2

/2

z

(a) Original geometry vC qA

A, A′

eAB B, B′

qB

C′ (b) Deformed shape

Figure 3.1 Deformation of a statically determinate member.

Provided that deﬂections are small and that simple beam theory is applicable, the slope θ and deﬂection v at any point z along the member are obtained by integrating the curvature κ(z) along the member as follows: θ=

κ(z) dz

(3.4)

v=

κ(z) dz dz

(3.5)

Eqs 3.4 and 3.5 are quite general and apply to both elastic and inelastic material behaviour. If the axial strain and curvature are calculated at any time after loading at a preselected number of points along the member shown in Fig 3.1 and if a reasonable variation of strain and curvature is assumed between adjacent points, it is a simple matter of geometry to determine the deformation of the member. For convenience, some simple equations are given below for the determination of the deformation of a single span and of a cantilever. If the axial strain εa and the curvature κ are known at the mid-span and at each end of the member shown in Fig 3.1 (i.e. at supports A and B and at point C), the axial deformation eAB , the slope at each support θA and θB and the deﬂection at mid-span vC are given by Eqs 3.6 and 3.7. For a linear variation of strain and curvature: eAB =

(εaA + 2 εaC + εaB ) 4

2 (κA + 4 κC + κB ) 48 θA = (5 κA + 6 κC + κB ) 24 θB = − (κA + 6 κC + 5 κB ) 24

vC =

(3.6a) (3.6b) (3.6c) (3.6d)

Design for serviceability

51

For a parabolic variation of strain and curvature: eAB =

(εaA + 4 εaC + εaB ) 6

(3.7a)

vC =

2 (κA + 10 κC + κB ) 96

(3.7b)

θA =

(κA + 2 κC ) 6

(3.7c)

θB = −

(2κC + κB ) 6

(3.7d)

In addition to the simple span shown in Fig. 3.1, Eqs 3.6 and 3.7 also apply to any member in a statically indeterminate frame, provided the strain and curvature at each support and at mid-span are known. Consider the ﬁxed-end cantilever shown in Fig. 3.2. If the curvatures at A, B and C are known, then the slope and deﬂection at the free end of the member are given by Eqs 3.8 and 3.9. For a linear variation of curvature: θC = − (κA + 2κB + κC ) 4 vC = −

(3.8a)

2 (5κA + 6 κB + κC ) 24

(3.8b)

For a parabolic variation of curvature: θC = − (κA + 4κB + κC ) 6 vC = −

(3.9a)

2 (κA + 2κB ) 6

(3.9b)

If the curvatures at the ﬁxed and free ends of the cantilever only are known (i.e. at A and C), then the slope and deﬂection at the free end C are given by Eqs 3.10 and 3.11.

A

B

C vC qC

Figure 3.2 Deformation of a ﬁxed-end cantilever.

52 Design for serviceability For a linear variation of curvature: θC = −

(κA + κC ) 2

(3.10a)

vC = −

2 (2κA + κC ) 6

(3.10b)

For a parabolic variation of curvature (typical of what occurs in a uniformly loaded cantilever): θC = −

(κA + 2κC ) 3

(3.11a)

vC = −

2 (κA + κC ) 4

(3.11b)

3.6.2 Load versus deﬂection response of a reinforced concrete member The short-term or instantaneous deformation of a cracked reinforced concrete crosssection subjected to combined bending and axial force can be readily determined using simple modular ratio theory (Section 3.6.3). After cracking, the properties of both the fully-cracked section and the uncracked section are often combined empirically to model tension stiffening and to approximate the average properties of the cracked region. Consider the load-deﬂection response of a simply-supported, singly reinforced concrete beam or one-way slab shown in Fig. 3.3. At loads less than the cracking load, Pcr , the member is uncracked and behaves homogeneously and elastically. The slope of the load-deﬂection plot (OA in Fig. 3.3) is proportional to the second moment of area of the uncracked transformed section, Iuncr . The member ﬁrst cracks at Pcr when the extreme ﬁbre tensile stress in the concrete at the section of maximum moment reaches the ﬂexural tensile strength of the concrete, fct.f . There is a sudden change in the local stiffness at, and immediately adjacent to, this ﬁrst crack. At the section containing the crack, the ﬂexural stiffness drops signiﬁcantly, but the rest of the member remains uncracked. As load increases, more cracks form and the average ﬂexural stiffness of the entire member decreases. If the tensile concrete in the cracked regions of the beam carried no stress, the load-deﬂection relationship would follow the dashed line ACD. If the average extreme ﬁbre tensile stress in the concrete remained at fct.f after cracking, the load-deﬂection relationship would follow the dashed line AE. In reality, the actual response lies between these extremes and is shown in Fig. 3.3 as the solid line AB. The difference between the actual response and the zero tension response is the tension stiffening effect (that reduces the instantaneous deﬂection by δ as shown). Tension stiffening is the contribution of the intact tensile concrete between the cracks to the post-cracking stiffness of the member. At each crack, the tensile concrete carries no stress, but as the distance from the crack increases, the tensile stress in the concrete increases due to the bond between the concrete and the tensile reinforcement. As the load increases, the average tensile stress in the concrete reduces as more cracks develop and, when the crack pattern is fully developed and the number of cracks has stabilised, the actual response becomes approximately parallel to the no tension response (OD in Fig. 3.3). For slabs containing small quantities of tensile reinforcement

Design for serviceability Deflection assuming no cracking

Load

Tension stiffening, dD E

B

53

D

Actual response

Pservice

Pcr

Concrete carries no tension anywhere A

C

Concrete carries no tension in the cracked regions Deflection O

Figure 3.3 Typical load versus deﬂection relationship.

(typically in ﬂoor slabs Ast /bd < 0.005), tension stiffening may be responsible for more than 50 per cent of the stiffness of the cracked member at service loads and δ remains signiﬁcant up to and beyond the point where the steel yields and the ultimate load is approached. Figure 3.4a shows an elevation of a singly reinforced concrete ﬂexural member subjected to a uniform bending moment M of sufﬁcient magnitude to establish the primary ﬂexural cracks. The variation of stress in the tensile reinforcement along the member is shown in Fig. 3.4b and the variation of tensile stress in the concrete at the steel level is shown in Fig. 3.4c. Over a gauge length containing several cracks, the average concrete tensile stress σc.avg at typical in-service levels of applied moment is a signiﬁcant percentage of the tensile strength of the concrete. The keys to predicting the instantaneous deﬂection are ﬁrst to evaluate the load required to cause ﬁrst cracking or, more precisely, the moment to cause ﬁrst cracking at the critical cross-section, and secondly to model tension stiffening accurately. Both of these tasks are not straightforward. Restraint to shrinkage provided by the bonded reinforcement and restraint to shrinkage at the member’s ends can cause signiﬁcant tension in the concrete in the ﬁrst few days after casting. Cracking may therefore occur at loads far less than that required to produce an extreme ﬁbre tensile stress equal to the modulus of rupture fct.f in a member without shrinkage. One commonly used approach for modelling tension stiffening in deﬂection calculations involves determining an average effective second moment of area (Ief ) for a cracked member. For a prismatic member, the effective second moment of area after cracking is less than the second moment of area of the uncracked transformed section (Iuncr ) and greater than the second moment of area of the fully-cracked crosssection (Icr ). Several different empirical equations are available for Ief , including the well-known equation developed by Branson (Ref. 17) that is included in ACI 318-08. A modiﬁed and signiﬁcantly more realistic version of Branson’s equation is speciﬁed in AS3600-2009. Another model for Ief was recently proposed by Bischoff (Ref. 24) and may be derived from the method speciﬁed in Eurocode 2 for

54 Design for serviceability Primary cracks M

M

ho Reinforcement (a) Elevation

sst.max

(b) Stress in tensile reinforcement

sc.avg (c) Tensile stress in concrete at steel level

Figure 3.4 Stress distributions at the steel level in a cracked reinforced concrete member.

the calculation of deﬂection. These approaches are presented and reviewed in the following sub-sections. 3.6.3 Modular ratio theory The second moment of area of a reinforced concrete cross-section is conventionally calculated using linear elastic analysis with the following assumptions: (i) plane sections remain plane (i.e. the strain distribution is linear); (ii) perfect bond exists between the reinforcement and the concrete; and (iii) the stress-strain relationships for concrete and steel are linear and elastic. The steel reinforcement is transformed into an equivalent area of concrete by multiplying the reinforcement area by the modular ratio n (where n = Es /Ec ) and the properties of the cross-section are determined using the principles of mechanics of solids. After cracking, the concrete in tension is assumed to carry no stress. This simple procedure is often called modular ratio theory and it is used to calculate the second moment of area of the section before and after cracking. In itself, it does not account for tension stiffening and does not include the time-dependent deformations caused by creep and shrinkage. Figure 3.5 shows the strains, stresses and resultant forces on a cracked, singly reinforced, rectangular cross-section subjected to an applied moment M. With regard to the stresses and deformations, there are two unknowns – the top ﬁbre compressive strain εtop and the depth to the neutral axis dn = kd. The depth to the neutral axis may be determined by equating the resultant compressive and tensile forces (i.e. by enforcing the requirement of equilibrium of longitudinal forces): C=T 0.5 σtop b kd = σst Ast

Design for serviceability b

kd/3 etop

stop

dn= kd

D

d N

55

A

C = ½stop b kd f = d(1−k/3)

M (1–k)d Ast

(a) Cross-section

est

(b) Strains

T = sst Ast

sst

(c) Stresses

(d) Forces

Figure 3.5 Strains, stresses and forces on a cracked section in bending.

and, assuming linear-elastic stress-strain laws for the reinforcement and the compressive concrete, this becomes: 0.5k =

εst Es Ast εst σst Ast = = nρ εtop Ec bd εtop σtop bd

(3.12)

where ρ is the tensile reinforcement ratio, Ast /bd. Compatibility requires that the strain diagram is linear and therefore: (1 − k)d 1 − k εst = = εtop kd k

(3.13)

Substituting Eq. 3.13 into Eq. 3.12 gives: 0.5k =

1−k nρ k

and solving this quadratic equation for k gives: k = (nρ)2 + 2nρ − nρ

(3.14)

It should be noted that k (and hence the depth to the neutral axis kd) depends only on the modular ratio n and the reinforcement ratio ρ and is independent of the applied moment M. The depth to the neutral axis remains constant after cracking as the moment increases, until either the concrete compressive stress distribution becomes curvilinear or the reinforcing steel yields. With k determined from Eq. 3.14, the top ﬁbre concrete stress σtop and the steel stress σst may be found from the moment equilibrium equation: M = C f = T f = ½σtop b kd2 (1 − k/3) = σst Ast d(1 − k/3) and hence σtop =

2M M and σst = Ast d(1 − k/3) b kd 2 (1 − k/3)

(3.15)

56 Design for serviceability Clearly, the stresses in both the concrete and the steel are linear functions of the applied moment M. With the stress and strain distributions established, the ﬂexural rigidity of the cracked section (Ec Icr ) may be obtained from the curvature (i.e. the slope of the strain diagram) as follows: εtop σtop M 2M = = = Ec Icr kd Ec kd Ec bk2 d 3 (1 − k/3)

(3.16)

From Eq. 3.16, the second moment of area of the cracked section is: Icr = ½ b d 3 k2 (1 − k/3)

(3.17)

For convenience, values of the neutral axis parameter k and the cracked second moment of area Icr of singly reinforced rectangular sections are given in Table 3.6. Table 3.6 Neutral axis depth (kd) and second moment of area (Icr = λbd3 ) for singly reinforced rectangular sections (n = Es /Ec ) ρ = Ast /bd

0.002 0.0025 0.003 0.0035 0.004 0.0045 0.005 0.0055 0.006 0.0065 0.007 0.0075 0.008 0.0085 0.009 0.0095 0.010 0.011 0.012 0.013 0.014 0.015 0.016 0.017 0.018 0.019 0.020

n=4

n=5

n=6

n=7

n=8

n=9

n = 10

k

λ

k

λ

k

λ

k

λ

k

λ

k

λ

k

λ

0.119 0.132 0.143 0.154 0.164 0.173 0.181 0.189 0.196 0.204 0.210 0.217 0.223 0.229 0.235 0.240 0.246 0.256 0.266 0.275 0.283 0.292 0.299 0.307 0.314 0.321 0.328

0.0068 0.0083 0.0098 0.0112 0.0127 0.0140 0.0154 0.0167 0.0180 0.0193 0.0206 0.0218 0.0230 0.0242 0.0254 0.0266 0.0277 0.0299 0.0321 0.0343 0.0363 0.0384 0.0404 0.0423 0.0442 0.0461 0.0479

0.132 0.146 0.159 0.170 0.181 0.191 0.200 0.209 0.217 0.225 0.232 0.239 0.246 0.252 0.258 0.264 0.270 0.281 0.292 0.301 0.311 0.319 0.328 0.336 0.344 0.351 0.358

0.0083 0.0102 0.0119 0.0137 0.0154 0.0170 0.0187 0.0202 0.0218 0.0233 0.0248 0.0263 0.0277 0.0291 0.0305 0.0319 0.0332 0.0358 0.0384 0.0408 0.0433 0.0456 0.0479 0.0501 0.0523 0.0544 0.0565

0.143 0.159 0.173 0.185 0.196 0.207 0.217 0.226 0.235 0.243 0.251 0.258 0.266 0.272 0.279 0.285 0.292 0.303 0.314 0.325 0.334 0.344 0.353 0.361 0.369 0.377 0.384

0.0098 0.0119 0.0140 0.0161 0.0180 0.0199 0.0218 0.0236 0.0254 0.0271 0.0288 0.0305 0.0321 0.0337 0.0353 0.0369 0.0384 0.0413 0.0442 0.0470 0.0497 0.0523 0.0548 0.0573 0.0597 0.0621 0.0644

0.154 0.170 0.185 0.198 0.210 0.221 0.232 0.242 0.251 0.260 0.268 0.276 0.283 0.291 0.298 0.304 0.311 0.323 0.334 0.345 0.355 0.365 0.374 0.383 0.392 0.400 0.407

0.0112 0.0137 0.0161 0.0183 0.0206 0.0227 0.0248 0.0268 0.0288 0.0308 0.0327 0.0345 0.0363 0.0381 0.0399 0.0416 0.0433 0.0465 0.0497 0.0527 0.0557 0.0585 0.0613 0.0640 0.0667 0.0692 0.0717

0.164 0.181 0.196 0.210 0.223 0.235 0.246 0.256 0.266 0.275 0.283 0.292 0.299 0.307 0.314 0.321 0.328 0.341 0.353 0.364 0.374 0.384 0.394 0.403 0.412 0.420 0.428

0.0127 0.0154 0.0180 0.0206 0.0230 0.0254 0.0277 0.0299 0.0321 0.0343 0.0363 0.0384 0.0404 0.0423 0.0442 0.0461 0.0479 0.0514 0.0548 0.0581 0.0613 0.0644 0.0674 0.0703 0.0731 0.0758 0.0785

0.173 0.191 0.207 0.221 0.235 0.247 0.258 0.269 0.279 0.289 0.298 0.306 0.314 0.322 0.330 0.337 0.344 0.357 0.369 0.381 0.392 0.402 0.412 0.421 0.430 0.438 0.446

0.0140 0.0170 0.0199 0.0227 0.0254 0.0280 0.0305 0.0329 0.0353 0.0376 0.0399 0.0421 0.0442 0.0463 0.0483 0.0503 0.0523 0.0561 0.0597 0.0633 0.0667 0.0699 0.0731 0.0762 0.0791 0.0820 0.0848

0.181 0.200 0.217 0.232 0.246 0.258 0.270 0.281 0.292 0.301 0.311 0.319 0.328 0.336 0.344 0.351 0.358 0.372 0.384 0.396 0.407 0.418 0.428 0.437 0.446 0.455 0.463

0.0154 0.0187 0.0218 0.0248 0.0277 0.0305 0.0332 0.0358 0.0384 0.0408 0.0433 0.0456 0.0479 0.0501 0.0523 0.0544 0.0565 0.0605 0.0644 0.0681 0.0717 0.0752 0.0785 0.0817 0.0848 0.0878 0.0908

Design for serviceability

57

3.6.4 AS 3600-2009 and ACI 318-08 3.6.4.1 Instantaneous deﬂection According to AS 3600-2009, the instantaneous or short-term deﬂection of a beam may be calculated using the mean value of the elastic modulus of concrete at the time of ﬁrst loading, Ec , together with the effective second moment of area of the span Ief . The effective second moment of area involves an empirical adjustment of the second moment of area of a cracked member to account for tension stiffening. For a given cross-section, Ief is calculated using Branson’s formula (Ref. 17): Ief = Icr + (Iuncr − Icr )(Mcr /Ms∗ )3 ≤ Ief ,max

(3.18)

where Icr is the second moment of area of the fully-cracked section (calculated using modular ratio theory); Iuncr is the second moment of area of the uncracked crosssection about its centroidal axis; Ms∗ is the maximum bending moment at the section, based on the short-term serviceability design load or the construction load; Mcr is the cracking moment given by: Mcr = Z(fct.f − σcs + P/A) + Pe ≥ 0.0

(3.19)

where Z is the section modulus of the uncracked section, referred to the extreme ﬁbre at which cracking occurs; fct.f is the characteristic ﬂexural tensile strength of concrete speciﬁed as fct.f = 0.6 fc ; P is the effective prestressing force (if any); e is the eccentricity of prestress measured to the centroidal axis of the section; A is the area of the uncracked cross-section; and σcs is the maximum shrinkage-induced tensile stress on the uncracked section at the extreme ﬁbre at which cracking occurs. In the absence of more reﬁned calculation, σcs may be taken as:

2.5ρw − 0.8ρcw ∗ σcs = (3.20) Es εsh 1 + 50ρw where ρw is the web reinforcement ratio for the tensile steel (Ast + Apt )/bw d; ρcw is the web reinforcement ratio for the compressive steel, if any (Asc /bw d); Ast is the area on non-prestressed tensile reinforcement; Apt is the area of prestressing steel in the tensile zone; Asc is the area of non-prestressed compressive reinforcement; Es is ∗ is the ﬁnal design shrinkage strain the elastic modulus of the steel in MPa; and εsh (after 30 years). For non-prestressed members, the maximum value of Ief at any crosssection in Eq. 3.18 is Ief ,max = Iuncr when ρ = Ast /bd ≥ 0.005 and Ief ,max = 0.6Iuncr when ρ < 0.005. For a simple-supported beam or slab, the value of Ief for the member is determined from the value of Ief at mid-span. For interior spans of continuous beams or slabs, Ief is half of the value of Ief at mid-span plus one quarter of the value of Ief at each support, while for end spans of continuous beams or slabs, Ief is half the mid-span value plus half the value at the continuous support. For a cantilever, Ief is the value of Ief at the support. The term σcs is introduced into Eq. 3.19 to allow for the reduction in the cracking moment that inevitably occurs because of the restraint to shrinkage provided by the bonded tensile reinforcement. Shrinkage-induced tension often causes extensive

58 Design for serviceability time-dependent cracking, particularly in lightly loaded members. This time-dependent cracking may occur weeks and months after the member is ﬁrst loaded and must be accounted for if a meaningful estimate of deﬂection is required. Eq. 3.20 is based on the expression originally proposed by Gilbert (Ref. 26) for singly reinforced rectangular sections, where conservative values were assumed for the elastic modulus and the creep coefﬁcient of concrete and about 70 per cent of the ﬁnal shrinkage was considered in the calculation of Mcr . The expression was modiﬁed to accommodate the inclusion of compressive reinforcement (Ref. 27). The calculation of σcs for more general crosssections is discussed in detail in Ref. 28. Where appropriate, the additional tension that may arise due to restraint to shrinkage provided by the supports of a beam or slab should also be taken into account. The allowance for shrinkage-induced tension is particularly important in the case of lightly reinforced members (including slabs) where the tension induced by the full service moment alone might not be enough to cause cracking. In such cases, failure to account for shrinkage may lead to deﬂection calculations in which cracking is not adequately taken into account and this may lead to gross underestimates of the actual deﬂection. For heavily reinforced sections, the problem is not as signiﬁcant, because the service loads are usually well in excess of the cracking load and tension stiffening is not as signiﬁcant. ACI 318-08 also speciﬁes Eq. 3.18, except that the gross second moment of area, Ig , is used rather than Iuncr and, with Mcr given by Z (0.62 fc ), it does not include any allowance for shrinkage-induced tension or the loss of stiffness caused by cracking due to early shrinkage. For many slabs, cracking will occur within weeks of casting due to early drying shrinkage and temperature changes, often well before the slab is exposed to its full service loads. In a recent comparison of the instantaneous deﬂection predicted by ACI 318-08 and the measured deﬂections of lightly reinforced concrete slabs (Ref. 18), ACI 318-08 signiﬁcantly underestimated the instantaneous deﬂection after cracking of every slab and, for the very lightly reinforced slabs (ρ < 0.003), the deﬂection was grossly underestimated. In addition, ACI 318 does not model the abrupt change in direction of the moment-deﬂection response at ﬁrst cracking and does not predict the correct shape of the moment-deﬂection plot after cracking (Ref. 18). 3.6.4.2 Time-dependent deﬂection For the calculation of long-term deﬂection, one of two approaches is speciﬁed in AS 3600-2009. For reinforced or prestressed beams, the creep and shrinkage deﬂections can be calculated separately (using the material data speciﬁed in the standard and the principles of mechanics). Alternatively, for reinforced concrete beams and slabs, the additional long-term deﬂection caused by creep and shrinkage may be crudely approximated by multiplying the short-term or immediate deﬂection caused by the sustained load by a multiplier kcs given by: kcs = [2 − 1.2(Asc /Ast )] ≥ 0.8

(3.21)

where Asc is the area of steel in the compressive zone of the cracked section between the neutral axis and the extreme compressive ﬁbre and the ratio Asc /Ast is taken at mid-span for a simple or continuous span and at the support for a cantilever.

Design for serviceability

59

ACI 318-08 also speciﬁes that unless a more comprehensive analysis is undertaken the additional long-term deﬂection resulting from the creep and shrinkage of ﬂexural members may be determined by multiplying the immediate deﬂection caused by the sustained load by a multiplier λ given by: λ =

ξ (1 + 50Asc /bd)

(3.22)

where Asc /bd is taken at mid-span for a simple or continuous span and at the support for a cantilever; and the time-dependent factor ξ depends on the duration of loads, with ξ = 2.0 for 5 years or more; ξ = 1.4 for 1 year; ξ = 1.2 for 6 months; and ξ = 1.0 for 3 months. The use of a deﬂection multiplier (kcs or λ ) to calculate time-dependent deﬂections is simple and convenient and, provided the section is initially cracked under shortterm loads, it may provide a ‘ball-park’ estimate of the ﬁnal deﬂection. However, to calculate the shrinkage-induced deﬂection by multiplying the load-induced short-term deﬂection by a long-term deﬂection multiplier is fundamentally incorrect. Shrinkage can cause signiﬁcant deﬂection even in unloaded members. The approach ignores many of the factors that inﬂuence the ﬁnal deﬂection, including the creep and shrinkage characteristics of the concrete, the environment and the age at ﬁrst loading. At best, it must be seen as providing a very approximate estimate. At worst, it is misleading and not worth the time involved in making the calculation. In addition, when using the ACI 318-08 multiplier, no account is taken of the loss of stiffness caused by shrinkageinduced cracking at any stage of the calculation procedure and, in the case of slabs, this may be very signiﬁcant. It is, however, not too much more complicated to calculate long-term creep and shrinkage deﬂections separately and this is the subject of much of the rest of this book. A recently proposed simpliﬁed method for deﬂection calculation that does calculate the creep and shrinkage deﬂections separately (and more accurately) is outlined in Section 3.6.6.

Example 3.2 The ﬁnal long-term deﬂection (vC )max at the mid-point C in the end span of a continuous one-way slab is to be calculated using the simpliﬁed procedures in AS 3600-2009 and ACI 318-08. The slab is 180 mm thick. The span is = ef = 5.0 m, the dead load g = 2.0 kPa + self-weight = 6.4 kPa, and the live load is q = 3.0 kPa. The short-term expected live load is q1 = 2.1 kPa and the sustained part of the live load is q2 = 1.2 kPa. The deﬂection requirement is that (vC )max ≤ ef /250 = 20 mm. = 0.6 f = 3.0 MPa The concrete and steel strengths are fc = 25 MPa, fct.f c and fy = 500 MPa. The elastic moduli for concrete and steel are Ec = 26,700 MPa and Es = 200,000 MPa, and the modular ratio is therefore n = Es /Ec = 7.5. The ∗ = 0.0007 and the clear concrete ﬁnal long-term shrinkage strain is taken to be εsh cover to the reinforcement is 20 mm.

60 Design for serviceability The bottom longitudinal reinforcement throughout the span consists of 12 mm diameter bars at 250 mm centres (Ast = 440 mm2 /m at d = 154 mm) and the top reinforcement at the interior support consists of 12 mm bars at 200 mm centres (Ast = 550 mm2 /m at d = 154 mm), as shown in Fig. 3.6. The reinforcement has been designed to provide adequate strength. Also shown in Fig. 3.6 is the bending moment diagram under the maximum uniformly distributed service load, wmax = g + q1 = 8.5 kPa. wmax = 8.5 kN/m2 N12@200 mm A A

C N12@250 mm B `=5m

(a) Elevation of end span

C −

D = 180 mm

+

B MB = −22.5 kNm/m

MC = +15.4 kNm/m

(b) Load and bending moment diagrams

Figure 3.6 Slab elevation, load and bending moment diagrams (Example 3.2).

AS3600-2009 Section at mid-span C The maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m. With Ast = 440 mm2 /m and d = 154 mm, the reinforcement ratio ρ = Ast /bd = 0.00286 and nρ = 0.0214, the centroidal axis of the uncracked transformed cross-section is 91.0 mm below the top surface and the second moment of area of the uncracked transformed section about its centroidal axis is Iuncr = 498 × 106 mm4 /m. The depth to the neutral axis for the cracked section is calculated using Eq. 3.14: k=

(0.0214)2 + 2 × 0.0214 − 0.0214 = 0.187

and therefore dn = kd = 28.7 mm. The second moment of area of the fullycracked transformed section, Icr , is next obtained from Eq. 3.17 as: Icr = ½b d 3 k2 (1 − k/3) = 59.6 × 106 mm4 /m. The bottom ﬁbre section modulus of the uncracked section is Z = Iuncr /yb = 5.59 × 106 mm3 /m. From Eq. 3.20, the shrinkage-induced tension in the bottom ﬁbre of the uncracked section is: σcs =

2.5 × 0.00286 × 2 × 105 × 0.0007 = 0.875 MPa 1 + 50 × 0.00286

Design for serviceability and the time-dependent cracking moment is obtained from Eq. 3.19 is: Mcr = 5.59 × 106 (3.00 − 0.875) × 10−6 = 11.9 kNm/m From Eq. 3.18, the effective second moment of area at mid-span is: (Ief )C = 59.6 × 106 + (498 × 106 − 59.6 × 106 )(11.9/15.4)3 = 261 × 106 mm4 /m Section at continuous B The maximum in-service moment at support B is Ms∗ = −22.5 kNm/m. At this critical section, Ast = 550 mm2 /m, d = 154 mm, ρ = 0.00357 and nρ = 0.0268. The section properties calculated as above are Iuncr = 500 × 106 mm4 /m, k = 0.206, and Icr = 72.2 × 106 mm4 /m. From Eq. 3.20, σcs = 1.06 MPa and the cracking moment is Mcr = 10.9 kNm/m. From Eq. 3.18, (Ief )B = 121 × 106 mm4 /m. For entire span The average effective second moment of area for the entire end span is taken as the average of the values at mid-span and at the continuous support. That is: Ief = 0.5 × ((Ief )C + (Ief )B ) = 0.5 × (261 × 106 + 121 × 106 ) = 191 × 106 mm4 /m Instantaneous deﬂection Assuming a uniform average rigidity for the span of Ec Ief , the instantaneous curvatures at the sections at mid-span and at the continuous support under the full service load after the effects of all cracking have been included are: (κi )C =

Ms∗ 15.4 × 106 = = 3.02 × 10−6 mm−1 Ec Ief 26,700 × 191 × 106

and (κi )B = −4.41 × 10−6 mm−1 The instantaneous deﬂection at mid-span due to the full service load after accounting for all load and shrinkage-induced cracking is obtained from Eq. 3.7b as: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 3.02 × 10−6 − 4.41 × 10−6 ) = 6.7 mm 96

61

62 Design for serviceability Time-dependent deﬂection In this example, the sustained load is wsus = g + q2 = 7.6 kPa. The instantaneous deﬂection due to the sustained loads is therefore: (vC )i.sus = (vC )i.max (wsus /wmax ) = 6.0 mm With no compressive reinforcement, the time-dependent deﬂection multiplication factor given by Eq. 3.21 is kcs = 2.0 and the time-dependent deﬂection at mid-span is: (vC )time = kcs (vC )i.sus = 2.0 × 6.0 = 12.0 mm The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is the sum of the instantaneous deﬂection due to the maximum service load and the time-dependent deﬂection due to creep and shrinkage and is given by: (vC )max = (vC )i.max + (vC )time = 6.7 + 12.0 = 18.7 mm = span/267 Discussion According to AS3600-2009, this slab will deﬂect a little less than the maximum deﬂection limit of span/250 and so the slab is just serviceable. A slightly thinner slab may be possible with the inclusion of some compressive reinforcement in the positive moment region. It is of interest to note that the deemed to comply maximum span-to-depth ratio in AS 3600-2009 is more conservative requiring minimum slab thickness of 207 mm, if deﬂections were not to be checked by calculation (see Example 3.1).

ACI318-08 Section at mid-span C The second moment of area of the gross cross-section is Ig = 486 × 106 mm4 /m. As calculated previously, with Ast = 440 mm2 /m and d = 154 mm, the second moment of area of the fully-cracked transformed section is Icr = 59.6 × 106 mm4 /m. The bottom ﬁbre section modulus of the gross section is Z = Ig /yb = 5.4 × 106 mm3 /m and the cracking moment is Mcr = Z(0.62 fc ) = √ 5.4 × 106 (0.62 25) × 10−6 = 16.7 kNm/m. According to ACI 318-08, with Ms∗ = 15.4 kNm/m, the slab will not crack in the positive moment region at any stage throughout its life and (Ief )C = Ig = 486 × 106 mm4 /m – a conclusion that experience would suggest is unsupportable. Section at continuous support B With Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d= 154 mm, Icr = 72.2×106 mm4 /m and Mcr = 16.7 kNm/m, Eq. 3.18 gives (Ief )B = 243 × 106 mm4 /m.

Design for serviceability For entire span According to ACI 318-08, the average effective second moment of area for the entire span may be taken as either the value at mid-span or the average of the values obtained at the positive and negative moment regions. For this typical example, taking the value at mid-span would be unconservative (and unwise), as the effects of any cracking would be completely ignored. Assuming that Ief is the average of the values at mid-span and at the continuous support gives Ief = 364 × 106 mm4 /m. Instantaneous deﬂection Assuming a uniform average rigidity for the span of Ec Ief , the instantaneous curvatures at the section at mid-span and at the continuous support under the full service load are (κi )C = 1.58 × 10−6 mm−1 and (κi )B = −2.31 × 10−6 mm−1 . From Eq. 3.7b, the instantaneous deﬂection at mid-span due to the full service load is: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 1.58 × 10−6 − 2.31 × 10−6 ) = 3.5 mm 96

Time-dependent deﬂection In this example, (vC )i.sus = (vC )i.max (wsus /wmax ) = 3.1 mm and with no compressive reinforcement, the time-dependent deﬂection multiplication factor given by Eq. 3.22 for a load duration of more than 5 years is λ = 2.0 and the time-dependent deﬂection at mid-span is: (vC )time = λ (vC )i.sus = 2.0 × 3.1 = 6.2 mm The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.max + (vC )time = 3.5 + 6.2 = 9.7 mm = span/515 Discussion According to ACI 318-08, the maximum ﬁnal long-term deﬂection of this 180 mm thick slab is less than half of that calculated by AS 3600-2009 and a signiﬁcantly thinner slab would be possible if the maximum ﬁnal deﬂection were to be limited to span/250. Clearly, the loss of stiffness due to shrinkageinduced cracking is ignored by ACI 318-08. Comparison of the ACI 318-08 predictions with the observed deﬂections in real slabs conﬁrms that often this method grossly underestimates deﬂection.

63

64 Design for serviceability By contrast, the minimum thickness speciﬁed for this slab in ACI 318-08 is 230 mm (see Example 3.1) and the selection of a slab thickness that met this requirement would be a very conservative design decision.

3.6.5 Eurocode 2 3.6.5.1 Instantaneous curvature An alternative approach for the calculation of deﬂection in a cracked reinforced concrete member is speciﬁed in Eurocode 2 (Ref. 6). This approach involves the calculation of the curvature at particular cross-sections and then twice integrating the curvatures along the member to obtain its deﬂection. The instantaneous curvature at a section after cracking, κ, is calculated as a weighted average of the values calculated on a fully-cracked section (κcr ) and on an uncracked section (κuncr ) as follows: κ = ζ κ cr + (1 − ζ )κuncr

(3.23)

where ζ is a distribution coefﬁcient that accounts for the moment level and the degree of cracking and, for members containing deformed bars, is given by: ζ = 1−β

σsr σs

2 (3.24a)

where β is a coefﬁcient to account for the effects of duration of loading or repeated loading on the average deformation and equals 1.0 for a single, short-term load and 0.5 for sustained loading or for many cycles of repeated loading; σsr is the stress in the tensile reinforcement at the load causing ﬁrst cracking that is calculated by ignoring concrete in tension and ignoring any shrinkage-induced tension; σs is stress in the reinforcement at the load under consideration that is calculated by ignoring concrete in tension; κcr is the curvature at the section calculated by ignoring concrete in tension; and κuncr is the curvature on the uncracked transformed section. If the compressive concrete and the reinforcement are both linear and elastic, the ratio σsr /σs in Eq. 3.24a can be replaced by Mcr /Ms∗ and therefore: ζ = 1−β

Mcr Ms∗

2 (3.24b)

The cracking moment Mcr is the moment required to produce an extreme ﬁbre tensile stress equal to the mean uniaxial tensile strength of concrete, fctm . For a reinforced concrete section in pure bending Mcr = Zfctm , where Z is the section modulus of the uncracked section, referred to the extreme ﬁbre at which cracking occurs, and fctm = 0.3(fc )2/3 when fc ≤ 50 MPa. The introduction of β = 0.5 in Eqs 3.24 for long-term deﬂection calculations is tantamount to reducing the cracking moment by about 30 per cent and is a crude way of accounting for shrinkage-induced tension and time-dependent cracking.

Design for serviceability

65

3.6.5.2 Time-dependent curvature For sustained loads, Eurocode 2 speciﬁes that the total load-induced deformation including creep may be calculated by using an effective modulus for concrete, Ee , given by: Ee =

Ec 1 + ϕ(∞, τ )

(3.25)

where ϕ(∞, τ ) is the creep coefﬁcient at time inﬁnity due to a load ﬁrst applied at time τ . The shrinkage-induced curvature κsh is obtained from the following expression: κsh = εsh ne

S I

(3.26)

where εsh is the free shrinkage strain; ne is the effective modular ratio (Es /Ee ); S is the ﬁrst moment of area of the reinforcement about the centroid of the section; and I is the second moment of area of the section. S and I and the corresponding curvatures should be calculated for both the uncracked condition and for the fully-cracked condition, and the ﬁnal average shrinkage-induced curvature in the cracked region is then calculated using Eq. 3.23.

Example 3.3 Using the Eurocode 2 approach, the ﬁnal long-term deﬂection (vC )max is to be calculated at the mid-point C in the end span of the one-way slab of Example 3.2 that is illustrated in Fig. 3.6. For convenience, details of the slab are included here: slab thickness, D = 180 mm; span = ef = 5.0 m; clear cover = 20 mm; dead load (including self-weight), g = 6.4 kPa; live load, q = 3.0 kPa; short-term expected live load, q1 = 2.1 kPa; sustained part of the live load, q2 = 1.2 kPa; the deﬂection requirement, (vC )max ≤ ef /500 = 20 mm; and the reinforcement details are outlined in Example 3.2. The material properties are: fc = 25 MPa; ∗ = fy = 500 MPa; Ec = 26,700 MPa; Es = 200,000 MPa; n = Es /Ec = 7.5; εsh 0.0007 and the ﬁnal creep coefﬁcient is ϕ ∗ (τ ) = 2.5. The mean uniaxial tensile strength of concrete is fctm = 0.3(fc )2/3 = 2.57 MPa.

Instantaneous deﬂection – Eurocode 2 Section at mid-span C As given in Example 3.2, the maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m. With Ast = 440 mm2 /m and d = 154 mm, the second moments of area of the uncracked transformed section and the fully-cracked transformed section are Iuncr = 498 × 106 mm4 /m and Icr = 59.6 × 106 mm4 /m, respectively. The uncracked and fully cracked curvatures are therefore κuncr = Ms∗ /Ec Iuncr = 1.16 × 10−6 mm−1 and κcr = Ms∗ /Ec Icr = 9.68 × 10−6 mm−1 , respectively.

66 Design for serviceability The cracking moment is Mcr = Zfctm = 5.59×106 ×2.57 ×10−6 = 14.34 kNm/m and, with β = 1.0 for short-term loading, the distribution coefﬁcient ζ is obtained from Eq. 3.24b: ζ = 1−β

Mcr Ms∗

2

= 1 − 1.0 × (14.34/15.4)2 = 0.133

The instantaneous curvature at mid-span is obtained from Eq. 3.23 as: (κi )C = 0.133 × 9.68 × 10−6 + (1 − 0.133) × 1.16 × 10−6 = 2.29 × 10−6 mm−1 Section at continuous support B At this critical section, Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d = 154 mm, Iuncr = 500 × 106 mm4 /m, Icr = 72.2 × 106 mm4 /m and Mcr = 14.46 kNm/m. The uncracked and fully-cracked curvatures at B are therefore κuncr = −1.68 × 10−6 mm−1 and κcr = −11.67 × 10−6 mm−1 , respectively. From Eq. 3.24b, ζ = 1 − 1.0 × (14.46/22.5)2 = 0.587 and the instantaneous curvature at B is: (κi )B = 0.587 × (−11.67 × 10−6 ) + (1 − 0.587) × (−1.68 × 10−6 ) = −7.54 × 10−6 mm−1 Deﬂection at mid-span The instantaneous deﬂection at mid-span due to the full service load is again obtained from Eq. 3.7b as: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 2.29 × 10−6 − 7.54 × 10−6 ) = 4.0 mm 96

of which, the instantaneous deﬂection due to the sustained load is 3.6 mm and the remaining instantaneous deﬂection due to the transient live load is (vC )i.(q1−q2) = 0.4 mm.

Time-dependent deﬂection due to sustained loads – Eurocode 2 The effective modulus of the concrete is obtained from Eq. 3.25 as: Ee =

26700 = 7630 MPa 1 + 2.5

and the effective modular ratio ne = Es /Ee = 26.2. With the effective modular ratio, the revised section properties of the uncracked and cracked transformed cross-sections at the mid-span and at the continuous support are required.

Design for serviceability Section at mid-span C With the reinforcement area transformed into an equivalent area of the softened concrete (due to creep) using the effective modular ratio, the second moments of area of the uncracked and fully-cracked cross-sections are Iuncr = 529 × 106 mm4 /m and Icr = 166 × 106 mm4 /m, respectively. Due to the sustained loads (wsus = g + q2 = 7.6 kPa), the moment at the section at mid-span is (MC )sus = 13.77 kNm/m and the time-dependent curvatures allowing for creep are κuncr = (MC )sus /Ee Iuncr = 3.41 × 10−6 mm−1 and κcr = (MC )sus /Ee Icr = 10.8 × 10−6 mm−1 . With Mcr = 14.34 kNm/m and with β = 0.5 for long-term loading, the distribution coefﬁcient ζ is obtained from Eq. 3.24b:

2 Mcr ζ = 1−β = 1 − 0.5 × (14.34/13.77)2 = 0.458 (MC )sus The long-term load-induced curvature at mid-span (including creep) is obtained from Eq. 3.23 as: (κsus )C = 0.458 × 10.8 × 10−6 + (1 − 0.458) × 3.41 × 10−6 = 6.82 × 10−6 mm−1 Section at continuous support B At this critical section, the revised second moments of area are Iuncr = 539 × 106 mm4 /m and Icr = 197 ×106 mm4 /m. The sustained moment at B is (MB )sus = −20.12 kNm/m and the time-dependent curvatures allowing for creep are κuncr = (MB )sus /Ee Iuncr = −4.89 × 10−6 mm−1 and κcr = −13.4 × 10−6 mm−1 . From Eq. 3.24b, ζ = 1 − 0.5 × (14.46/20.12)2 = 0.742 and, the long-term load-induced curvature at B is: (κsus )B = 0.742 × (−13.4 × 10−6 ) + (1 − 0.742) × (−4.89 × 10−6 ) = −11.2 × 10−6 mm−1 Deﬂection at mid-span The time-dependent deﬂection at mid-span due to the sustained loads plus creep is obtained from Eq. 3.7b as: (vC )sus = =

2 ((κsus )A + 10 (κsus )C + (κsus )B ) 96 50002 (0 + 10 × 6.82 × 10−6 − 11.2 × 10−6 ) = 14.8 mm 96

Time-dependent deﬂection due to shrinkage – Eurocode 2 Section at mid-span C As for the creep analysis, the second moments of area of the uncracked and fullycracked cross-sections are Iuncr = 529 × 106 mm4 /m and Icr = 166 × 106 mm4 /m,

67

68 Design for serviceability respectively, and the ﬁrst moment of area of the reinforcement about the centroidal axis of the uncracked and fully-cracked cross-sections are Suncr = 26.5 × 103 mm3 /m and Scr = 46.1 × 103 mm3 /m, respectively. The shrinkageinduced curvatures are obtained from Eq. 3.26: (κsh )uncr = εsh ne

Suncr = 0.92 × 10−6 mm−1 Iuncr

and (κsh )cr = εsh ne

Scr = 5.09 × 10−6 mm−1 Icr

With ζ = 0.458, as for in the creep analysis, the shrinkage-induced curvature at mid-span is obtained from Eq. 3.23 as: (κsh )C = 0.458 × 5.09 × 10−6 + (1 − 0.458) × 0.92 × 10−6 = 2.82 × 10−6 mm−1 At the supports At the discontinuous support A, the member is uncracked and so (κsh )A = 0.92 × 10−6 mm−1 . In the negative moment region, adjacent to support B, the slab contains both top and bottom reinforcement and Suncr = −6.2 × 103 mm3 /m, Iuncr = 588×106 mm4 /m, Scr = −46.9×103 mm3 /m and Icr = 204×106 mm4 /m. Therefore, from Eq. 3.26: (κsh )uncr = −0.19×10−16 mm−1 and (κsh )cr = −4.22× 10−6 mm−1 . With ζ = 0.742, Eq. 3.23 gives (κsh )B = −3.18 × 10−6 mm−1 . Shrinkage-induced deﬂection at mid-span An estimate of the shrinkage-induced deﬂection is obtained by assuming a parabolic distribution of shrinkage curvature between the end sections and mid-span. Eq. 3.7b gives: (vC )sh = =

2 ((κsh )A + 10 (κsh )C + (κsh )B ) 96 50002 (0.92 + 10 × 2.82 − 3.18) × 10−6 = 6.8 mm 96

The ﬁnal long-term deﬂection – Eurocode 2 The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.q1−q2 + (vC )sus + (vC )sh = 0.4 + 14.8 + 6.8 = 22.0 mm = span/227

Design for serviceability

69

Discussion This result is in reasonable agreement with the ﬁnal deﬂection calculated in Example 3.2 using AS 3600-2009, although a little more conservative. Unlike AS 3600-2009 (and ACI 318-08), the approach provides a rational consideration of the long-term deﬂection due to creep and shrinkage of the concrete. Of course, the ﬁnal deﬂection here is heavily dependent on input values of the creep coefﬁcient and the shrinkage strain of concrete – as is the case in real slabs. The use of the mean concrete tensile strength fctm instead of the ﬂexural strength indirectly compensates for the tension induced by restrained shrinkage (Ref. 24). It is of interest to note that deemed-to-comply maximum span-to-depth ratios in Eurocode 2 (Eqs 3.2) suggest that, if a slab thickness greater than 173 mm was selected (see Example 3.1), then the maximum ﬁnal long-term deﬂection will not exceed span/250 and deﬂections need not be calculated. This example suggests that this is not the case and that Eqs 3.2 cannot be relied on to guarantee adequate serviceability.

3.6.6 Recommended simpliﬁed approach It is well known that Branson’s Equation (Eq. 3.18) overestimates stiffness after cracking for members containing relatively small quantities of tensile reinforcement (Refs 18, 25 and 26). A much better model for Ief can be developed from the deﬂection calculation approach in Eurocode 2 (as outlined in Section 3.6.5). Substituting Eq. 3.24b into Eq. 3.23, the instantaneous curvature at a particular section in the cracked region of a member may be calculated from:

Mcr 2 Mcr 2 κ = 1−β κcr + β κuncr (3.27) Ms∗ Ms∗ Using the notation of Eq. 3.18, the curvatures in Eq. 3.27 are κ = Ms∗ /Ec Ief , κcr = Ms∗ /Ec Icr and κuncr = Ms∗ /Ec Iuncr and Eq. 3.27 can be re-expressed as:

∗

Ms∗ Mcr 2 Ms Mcr 2 Ms∗ = 1−β + β (3.28) Ec Ief Ms∗ Ec Icr Ms∗ Ec Iuncr Eq. 3.28 can be rearranged to give the following expression for Ief : Ief =

1−β 1−

Icr Icr Iuncr

Mcr Ms∗

2 ≤ Ief .max

(3.29)

This alternative expression for Ief was ﬁrst proposed by Bischoff (Ref. 25). 3.6.6.1 Instantaneous deﬂection The instantaneous curvature κi due to the service moment Ms∗ at a particular crosssection is κi = Ms∗ /Ec Ief , with Ief calculated from Eq. 3.29, where Icr is the second moment of area of the fully-cracked section about its centroidal axis; Iuncr is the

70 Design for serviceability second moment of area of the uncracked transformed cross-section about its centroidal axis; Ms∗ is the maximum bending moment at the section, based on the short-term serviceability design load or the construction load; Mcr is the cracking moment given by + P/Ag ) + Pe ≥ 0.0 Mcr = Z(fct.f

(3.30)

where Z is the section modulus of the uncracked section, referring to the extreme (= 0.6 f ) is the characteristic ﬂexural tensile ﬁbre at which cracking occurs; and fct.f c strength of concrete. An upper limit Ief .max is recommended for the value of Ief calculated from Eq. 3.29, where Ief .max = Iuncr when p = Ast /bd ≥ 0.005 and Ief .max = 0.6Iuncr when p < 0.005. For lightly reinforced members (where ρ < 0.005), the value of Ief is very sensitive to the calculated value of Mcr . The ratio Iuncr /Icr is large and the maximum in-service moment Ms∗ may be similar in magnitude to the cracking moment. An upper limit for Ief of 0.6Iuncr is imposed on such members, because failure to account for cracking due to unanticipated shrinkage restraint, temperature gradients or construction loads can result in signiﬁcant underestimates of deﬂection. The term β in Eq. 3.29 is used to account for both shrinkage-induced cracking and the reduction in tension stiffening with time. Early shrinkage in the days and weeks after casting will cause tension in the concrete and a reduction in the cracking moment. As time progresses and the concrete continues to shrink, the level of shrinkage-induced tension increases in an uncracked member, further reducing the cracking moment. If shrinkage has not occurred before ﬁrst loading, the deﬂection immediately after loading may be calculated with β = 1.0. However, in practice, signiﬁcant shrinkage usually occurs before ﬁrst loading and β is less than 1.0. When calculating the shortterm or elastic part of the deﬂection, the following is recommended: β = 0.7 β = 0.5

at early ages (less than 28 days); and at ages greater than 6 months.

For long-term calculations, when the ﬁnal deﬂection is to be estimated, β = 0.5 should be used. The instantaneous deﬂection is calculated by assuming a uniform average rigidity for the span of Ec (Ief )av . For a simple-supported beam or slab, the average value (Ief )av for the span is determined from the value of Ief at mid-span. For interior spans of continuous beams or slabs, (Ief )av is taken to be half the mid-span value plus one quarter of the value at each support. For end spans of continuous beams or slabs, (Ief )av is taken to be half the mid-span value plus half the value at the continuous support. For a cantilever, (Ief )av is the value at the support. 3.6.6.2 Time-dependent creep-induced curvature The creep-induced curvature κcr (t) on a particular cross-section at any time t due to a sustained service load ﬁrst applied at age τ0 may be obtained from: κcr (t) = κsus,0

ϕ(t, τ0 ) α

(3.31)

Design for serviceability

71

where κsus,0 is the instantaneous curvature due to the sustained service loads; ϕ(t, τ0 ) is the creep coefﬁcient at time t due to load ﬁrst applied at age τ0 ; and α is a creep modiﬁcation factor that accounts for the effects of cracking and the braking action of the reinforcement on creep and may be estimated from either Eqs 3.32a, b or c (Refs 26 and 30). For a cracked reinforced concrete section in pure bending (Ief < Iuncr ), α = α1 , where:

α1 = 0.48ρ

−0.5

I 0.33 Asc 1.2 cr 1 + (125ρ + 0.1) Ief Ast

(3.32a)

For an uncracked reinforced or prestressed concrete section (Ief = Iuncr ), α = α2 , where: Asc (3.32b) α2 = 1.0 + 45ρ − 900ρ 2 1 + Ast and ρ = Ast /bdo ; Ast is the equivalent area of bonded reinforcement in the tensile zone at depth do (the depth from the extreme compressive ﬁbre to the centroid of the outermost layer of tensile reinforcement); and Asc is the area of the bonded reinforcement in the compressive zone between the neutral axis and the extreme compressive ﬁbre. The area of any bonded reinforcement in the tensile zone (including bonded tendons) not contained in the outermost layer of tensile reinforcement (i.e. located at a depth d1 less than do ) should be included in the calculation of Ast by multiplying that area by d1 /do . For the purpose of the calculation of Ast , the tensile zone is that zone that would be in tension due to the applied moment acting in isolation. For a cracked, partially prestressed section or for a cracked reinforced concrete section subjected to bending and axial compression, α may be taken as:

dn1 α = α2 + (α1 − α2 ) dn

2.4 (3.32c)

where dn is the depth of the intact compressive concrete on the cracked section and dn1 is the depth of the intact compressive concrete on the cracked section ignoring the axial compression and/or the prestressing force (i.e. the value of dn for an equivalent cracked reinforced concrete section in pure bending containing the same quantity of bonded reinforcement). 3.6.6.3 Time-dependent shrinkage-induced curvature The shrinkage-induced curvature on a reinforced concrete section is approximated by:

κsh =

kr εsh D

(3.33)

where D is the overall depth of the section; εsh is the shrinkage strain; and kr depends on the quantity and location of bonded reinforcement Ast and Asc , and may be estimated from Eqs 3.34a–d, as appropriate (Ref. 30).

72 Design for serviceability For a cracked reinforced concrete section in pure bending (Ief < Iuncr ), kr = kr1 , where:

Icr kr1 = 1.2 Ief

0.67 1 − 0.5

Asc Ast

D do

(3.34a)

For an uncracked cross-section (Ief = Iuncr ), kr = kr2 , where:

do Asc 1.3 −1 1− when ρ = Ast /bdo ≤ 0.01 0.5D Ast (3.34b)

1.3

do Asc kr2 = (40ρ + 0.35) when ρ = Ast /bdo > 0.01 (3.34c) −1 1− 0.5D Ast

kr2 = (100ρ − 2500ρ 2 )

In Eqs 3.34a, b and c, Asc is deﬁned as the area of the bonded reinforcement on the compressive side of the cross-section. This is a different deﬁnition to that provided under Eq. 3.32b. While bonded steel near the compressive face of a cracked crosssection that is at or below the neutral axis will not restrain compressive creep, it will provide restraint to shrinkage and will affect the shrinkage-induced curvature on a cracked section. For a cracked, partially prestressed section or for a cracked reinforced concrete section subjected to bending and axial compression, kr may be taken as: kr = kr2 + (kr1 − kr2 )

dn1 dn

(3.34d)

where dn and dn1 are as deﬁned after Eq. 3.32c. Eqs 3.32, 3.33 and 3.34 have been developed (see Ref. 30) as empirical ﬁts to results obtained from a parametric study of the creep- and shrinkage-induced changes in curvature on reinforced concrete cross-sections under constant sustained internal actions using the age-adjusted effective modulus method (AEMM) of analysis (as outlined subsequently in Chapter 5).

Example 3.4 Using the approach recommended above (Eqs 3.29–3.34), the ﬁnal long-term deﬂection (vC )max is to be calculated at the mid-point C in the end span of the one-way slab of Example 3.2 that was illustrated in Fig. 3.6. For convenience, details of the slab are included here: h = 180 mm; = ef = 5.0 m; clear cover = 20 mm; dead load (including self-weight), g = 6.4 kPa; live load, q = 3.0 kPa; short-term expected live load, q1 = 2.1 kPa; sustained live load, q2 = 1.2 kPa; and (vC )max ≤ ef /500 = 20 mm. The reinforcement details are outlined in Example 3.2 and shown in Fig. 3.6a; and the bending moment diagram under the maximum uniformly distributed service load, wmax = g + q1 = 8.5 kPa is shown in Fig. 3.6b.

Design for serviceability The material properties are fc = 25 MPa; fct.f 3.0 MPa; fy = 500 MPa; ∗ = 0.0007 and Ec = 26,700 MPa; Es = 200,000 MPa; n = Es /Ec = 7.5; εsh ∗ ϕ (τ ) = 2.5.

Instantaneous deﬂection Section at mid-span C The maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m and with Ast = 440 mm2 /m, d = 154 mm and p = 0.00286, the second moments of area of the uncracked transformed section and the fully-cracked transformed section are Iuncr = 498 × 106 mm4 /m and Icr = 59.6 × 106 mm4 /m, respectively. The = 5.59 × 106 × 3.0 × 10−6 = 16.8 kNm/m and, cracking moment is Mcr = Zfct.f for the calculation of immediate deﬂection due to loads applied at any time after shrinkage-induced cracking has occurred, take β = 0.5. The value of Ief for the section at mid-span is obtained from Eq. 3.29:

Ief =

59.6 × 106

1 − 0.5 1 −

59.6 × 106

498 × 106

16.8 15.4

6 4

2 = 125 × 10 mm /m

Section at continuous support B At this critical section, Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d = 154 mm, Iuncr = 500 × 106 mm4 /m, Icr = 72.2 × 106 mm4 /m, Mcr = 16.9 kNm/m and therefore: Ief =

72.2 × 106

72.2 × 106 1 − 0.5 1 − 500 × 106

16.9 22.5

6 4

2 = 95.3 × 10 mm /m

Short-term deﬂection at mid-span The average value (Ief )av for the span is taken as one half the value of Ief at mid-span plus half the value at the continuous support. That is (Ief )av = 0.5 (125 + 95.3) × 106 = 110 × 106 mm4 /m. The instantaneous curvature at midspan and at support B are (κi )C = Ms∗ /Ec (Ief )av = (15.4 × 106 )/(26,700 × 110 × 106 ) = 5.24 × 10−6 mm−1 and (κi )B = Ms∗ /Ec (Ief )av = (−22.5 × 106 )/(26,700 × 110 × 106 ) = −7.66 × 10−6 mm−1 , respectively. The instantaneous deﬂection at mid-span due to the full service load is obtained from Eq. 3.7b as: (vC )i. max = =

2 ((κi )A + 10 (κi )C + (κi )B ) 96 50002 (0 + 10 × 5.24 × 10−6 − 7.66 × 10−6 ) = 11.7 mm 96

73

74 Design for serviceability

Time-dependent deﬂection Creep The sustained service load is wsus = g + q2 = 7.6 kPa = 0.894wmax , and therefore the sustained moments at mid-span and at the continuous support are Msus = 13.8 kNm/m and −20.1 kNm/m, respectively. The instantaneous curvatures at mid-span and at the continuous support due to the sustained loads (κsus,0 = Msus /Ec Ief .av ) are therefore 4.68 × 10−6 mm−1 and −6.85 × 10−6 mm−1 , respectively. The creep modiﬁcation factor α for the sections at mid-span and at the continuous support are obtained from Eq. 3.32a as α = α1 = [0.48 × 0.00286−0.5 ] × [59.6 × 106 /125 × 106 ]0.33 = 7.0 and α = α1 = [0.48 × 0.00357−0.5 ] × [72.2 × 106 /95.3 × 106 ]0.33 = 7.3, respectively. For the cross-section at the continuous support, the bottom (compressive) steel is not located in the compressive zone of the cracked section and so Asc in Eq. 3.32a is zero. From Eq. 3.31 the ﬁnal creep-induced curvature at the mid-span C and at the continuous support B are (κcr )C = 4.68×10−6 ×2.5/7.0 = 1.67×10−6 mm−1 and (κcr )B = −6.85 × 10−6 × 2.5/7.3 = −2.35 × 10−6 mm−1 , respectively. From Eq. 3.7b, the creep-induced deﬂection is: (vC )cr = =

2 ((κcr )A + 10 (κcr )C + (κcr )B ) 96 50002 (0 + 10 × 1.67 × 10−6 − 2.35 × 10−6 ) = 3.7 mm 96

Shrinkage For the cracked cross-section at mid-span, Eq. 3.34a gives kr = kr1 = 1.2 × (59.6 × 106 /125 × 106 )0.67 × 180/154 = 0.85 and the shrinkage-induced curvature is given by Eq. 3.33, (κsh )C = 0.85×0.0007/180 = 3.32×10−6 mm−1 . For the cracked section at the continuous support, Asc = 440 mm2 /m in Eq. 3.34a and kr = kr1 = 1.2 × (72.2 × 106 /95.3 × 106 )0.67 × (1 − 0.5 × 440/550) × (180/154) = 0.70 and the shrinkage-induced curvature is given by Eq. 3.33: (κsh )B = −0.70 × 0.0007/180 = −2.72 × 10−6 mm−1 . For the uncracked, singlyreinforced section at support A, Eq. 3.34b gives kr = kr2 = (100 × 0.00286 − 2500 × 0.002862 ) × (154/90 − 1) = 0.19 and, from Eq. 3.33, (κsh )A = 0.19 × 0.0007/180 = 0.74 × 10−6 mm−1 . If shrinkage-induced deﬂection is obtained by assuming a parabolic distribution of shrinkage curvature between the end sections and mid-span, Eq. 3.7b gives: (vC )sh = =

2 ((κsh )A + 10 (κsh )C + (κsh )B ) 96 50002 (0.74 + 10 × 3.32 − 2.72) × 10−6 = 8.1 mm 96

Design for serviceability

75

The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.max + (vC )cr + (vC )sh = 11.7 + 3.7 + 8.1 = 23.5 mm = span/213 Discussion The ﬁnal deﬂection calculated here is similar to that calculated in Example 3.3 using the procedure in Eurocode 2. However, this is not necessarily the case in all situations. The procedure described in Section 3.6.6 is considered to be the most reliable of the simpliﬁed procedures presented in this chapter and will generally provide a conservative estimate of deﬂections.

3.7 Crack control 3.7.1 General Reinforced concrete elements crack wherever the tensile stress in the concrete reaches the tensile strength of the concrete. Tensile stress at any location in a concrete structure may be caused by a number of factors, including applied loads, restrained shrinkage, temperature changes, settlement of supports and so on. Cracks formed by axial tensile forces and restrained shrinkage (direct tension cracks) often penetrate completely through a member. Cracks caused by bending (ﬂexural cracks) occur at the tensile face when the extreme ﬁbre tensile stress reaches the tensile strength of the concrete. Flexural cracks propagate from the extreme tensile ﬁbre through the tensile zone and are arrested at or near the neutral axis. Flexural cracks increase in width as the distance from the tensile reinforcement increases and taper to zero width near the neutral axis. A linear relationship is generally assumed to exist between the crack width at the side or sofﬁt of a member and the distance from the bar. In general, the spacing between ﬂexural cracks is in the range 0.5 to 1.5 times the depth of the member. Many variables inﬂuence the width and spacing of cracks, including the magnitude and duration of loading, the quantity, orientation and distribution of the reinforcement, the cover to the reinforcement, the slip between the reinforcement and the concrete in the vicinity of the crack (that depends on the bond characteristics of the reinforcement), the deformational properties of the concrete (including its creep and shrinkage characteristics) and the size of the member. Considerable variations exist in the crack width from crack to crack and the spacing between adjacent cracks because of random variations in the properties of concrete. The control of cracking in concrete structures is usually achieved by limiting the stress in the bonded reinforcement crossing a crack to some appropriately low value and ensuring that the bonded reinforcement is suitably distributed within the tensile zone. The limit on the tensile steel stress imposed in design depends on the maximum acceptable crack width. Typical values for maximum acceptable crack widths were given in Table 3.2 in Section 3.4.2. If the maximum acceptable crack

76 Design for serviceability width is increased, the maximum permissible tensile steel stress also increases. Building codes usually specify maximum bar spacings for the bonded reinforcement and maximum concrete cover requirements. Some codes specify deterministic procedures for calculating crack widths, with the intention to control cracking by limiting the calculated crack width to some appropriately low value. However, current design procedures to control cracking using conventional steel reinforcement are often overly simplistic and fail to adequately account for the gradual increase in crack widths with time due to shrinkage. In Chapter 1, Section 1.3.3, the restraint provided to shrinkage by the bonded reinforcement in a reinforced concrete member was discussed, with the concrete compressing the reinforcement as it shrinks and the reinforcement imposing an equal and opposite tensile force on the concrete at the level of the steel (as shown in Fig. 1.14b). This internal tensile restraining force is often signiﬁcant enough to cause time-dependent cracking. In addition, the connections of a concrete member to other parts of the structure or to the foundations also provide restraint to shrinkage. The tensile restraining force that develops rapidly with time at the restrained ends of the member usually leads to cracking, often within days of the commencement of drying. In a restrained ﬂexural member, shrinkage also causes a gradual widening of ﬂexural cracks and a gradual build-up of tension in the uncracked regions that may lead to additional cracking. The inﬂuence of shrinkage on crack widths is not properly considered in the major building codes and is therefore not adequately considered in structural design. As a consequence, excessively wide cracks are a relatively common problem for many reinforced concrete structures. 3.7.2 Simpliﬁed code-oriented approaches for ﬂexural crack control Many simpliﬁed approaches for crack control in reinforced concrete are available in the literature. Some of the more commonly used methods are presented and evaluated here. 3.7.2.1 Gergely and Lutz (Ref. 31) Based on a statistical analysis of experimental data, Gergely and Lutz proposed the following expression for the maximum crack width w (mm) at the tensile face of a beam or slab containing deformed bars: w = 0.011

D − kd σst1 (c1 A)0.33 × 10−3 d − kd

(3.35)

where c1 is the concrete cover measured from the tensile face to the centre of the longitudinal bar closest to that face (mm); A is the concrete area surrounding each longitudinal bar and may be taken as the total effective area of the concrete in the tensile zone of the cross-section having the same centroid as the tensile reinforcement divided by the number of longitudinal bars (mm2 ); σst1 is the tensile steel stress at the crack (MPa); D is the overall depth of the cross-section; d is the effective depth deﬁned as the distance from the compressive edge of the cross-section to the centroid of the tensile reinforcement; and kd is the depth from the compressive edge to the neutral axis of the cracked section.

Design for serviceability

77

3.7.2.2 Frosch (Ref. 32) The following alternative expression for the maximum crack width w (mm) at the tensile face of a beam or slab containing deformed bars was proposed by Frosch: w=2

σst1 D − kd 2 c1 + (sb /2)2 Es d − kd

(3.36)

where sb is the maximum bar spacing (mm); and Es is the elastic modulus of the steel (MPa). 3.7.2.3 Eurocode 2 – 1992 (Ref. 5) According to the 1992 version of Eurocode 2, the design crack width may be calculated from:

σst1 σsr 2 1 − β1 β2 (3.37) w = β srm Es σst1 where β1 = 1.0 for deformed bars and 0.5 for plain bars; β2 = 1.0 for a single, shortterm load and 0.5 for repeated or sustained loading; σsr is the stress in the tensile reinforcement at the loading causing ﬁrst cracking calculated ignoring the concrete in tension; σst1 is the stress in the reinforcement at the loading under consideration calculated ignoring the concrete in tension; β is the ratio of the design crack width to the average crack width taken as β = 1.7 for load-induced cracking and, for cracking due to restrained shrinkage, β = 1.3 when the minimum dimension of the member is less than 300 mm and increases to β = 1.7 when the minimum dimension is 800 mm or greater; srm is the average crack spacing given by: srm = 50 + 0.25 k1 k2 db /ρeff

(3.38)

in which k1 is a coefﬁcient equal to 0.8 for deformed bars and 1.6 for plain round bars; k2 is a coefﬁcient that takes into account the form of the strain distribution on the cross-section and equals 0.5 for bending and 1.0 for direct tension; db is the average bar diameter for the tensile reinforcement; and ρeff is the effective reinforcement ratio, Ast /Ac.eff ; Ast is the area of tensile reinforcement; and Ac.eff is the effective area of the tensile concrete surrounding the tensile reinforcement of depth equal to 2.5 times the distance from the tension face of the section to the centroid of the tensile reinforcement (i.e. 2.5(D − d)), but not greater than (D − kd)/3 or D/2. 3.7.2.4 Eurocode 2 – 2004 (Ref. 6) In the 2004 version of Eurocode 2, the crack width in a reinforced concrete member is calculated from: w = sr,max (εsm − εcm )

(3.39)

where sr,max is the maximum crack spacing; εsm is the mean strain in the reinforcement at the design loads, including the effects of tension stiffening and any imposed

78 Design for serviceability deformations; εcm is the mean strain in the concrete between the cracks. The difference between the mean strain in the reinforcement and the mean strain in the concrete may be taken as: εsm − εcm =

fct,eff σst1 σst1 − kt (1 + n ρeff ) ≥ 0.6 Es Es ρeff Es

(3.40)

where kt is a factor that depends on the duration of load and equals 0.6 for shortterm loading and 0.4 for long-term loading; n is the modular ratio Es /Ec ; fct,eff is the mean value of the axial tensile strength of concrete at the time cracking is expected; ρeff (= As /Ac,eff ) and Ac,eff are deﬁned under Eq. 3.38. For reinforced concrete sections with bonded reinforcement ﬁxed at reasonably close centres, the maximum ﬁnal crack width may be calculated from: sr,max = 3.4c + 0.425 k1 k2 db /ρeff

(3.41)

in which c is the clear cover to the longitudinal reinforcement; and k1 and k2 are deﬁned under Eq. 3.38. Alternatively, cracking is deemed to be controlled by Eurocode 2 (2004) if the quantity of tensile reinforcement in a beam or slab is greater than the minimum value given in Eq. 3.42 and if either the bar diameter and/or the bar spacing is limited to the maximum values given in Tables 3.7 and 3.8, respectively. The minimum area of steel for crack control is As,min = kc fct,eff Act /fs

(3.42)

where kc depends on the stress distribution prior to cracking and equals 1.0 for pure tension and 0.4 for pure bending; Act is the cross-sectional area of concrete in the tensile zone, i.e. the area in tension just before the formation of the ﬁrst crack; and fs is the maximum stress permitted in the reinforcement immediately after crack formation and is the lesser of the yield stress fy and the value given in Table 3.7. If the area of steel in the tension zone exceeds the minimum value given by Eq. 3.42, cracking is deemed to be controlled if either Tables 3.7 or 3.8 are satisﬁed. The steel stress used in these tables is the steel stress on the cracked section due to the quasipermanent loads. Table 3.7 Maximum bar diameters db for crack control (Ref. 6) Steel stress (MPa)

160 200 240 280 320 360 400 450

Maximum bar diameter (mm) Crack width, w = 0.4 mm

Crack width, w = 0.3 mm

Crack width, w = 0.2 mm

40 32 20 16 12 10 8 6

32 25 16 12 10 8 6 5

25 16 12 8 6 5 4 –

Design for serviceability

79

Table 3.8 Maximum bar spacing for crack control (Ref. 6) Steel stress (MPa)

Maximum bar spacing (mm) Crack width, w = 0.4 mm

Crack width, w = 0.3 mm

Crack width, w = 0.2 mm

300 300 250 200 150 100

300 250 200 150 100 50

200 150 100 50 – –

160 200 240 280 320 360

3.7.2.5 ACI 318-08 (Ref. 4) For the control of ﬂexural cracking in beams and one-way slabs in normal exposure conditions, ACI 318-08 requires the following. (i) The area of tensile steel provided at every cross-section should be greater than Ast.min where: 0.25 fc Ast. min = bw d ≥ 1.4bw d/fy fy

(3.43)

(ii) The ﬂexural tensile reinforcement is well distributed within the tensile zone of the cross-section and the spacing of the reinforcing bars closest to the tensile face is less than that given by: s = 380

280 280 − 2.5c ≤ 300 σst1 σst1

(3.44)

where c is the smallest distance from the surface of the reinforcement to the tensile face (mm); σst1 is the calculated stress at the crack in the reinforcement closest to the tensile face at the maximum service load (MPa), but it is permissible to take σst1 = 0.67fy . For two-way slabs, ACI 318-08 requires that the spacing of the reinforcement in each direction in a solid slab not exceed two times the slab thickness.

Example 3.5 The maximum crack width determined using Eqs 3.35, 3.36, 3.37 and 3.39 are here compared with the measured maximum ﬁnal crack widths for 12 prismatic, one-way, singly reinforced concrete specimens (six beams and six slabs) that were tested by Gilbert and Nejadi (Ref. 35) under sustained service loads for periods in excess of 400 days. The specimens were simply-supported over a span of 3.5 m with cross-sections shown in Fig. 3.7. All specimens were cast from the same

80 Design for serviceability batch of concrete and moist cured prior to ﬁrst loading at age 14 days. Details of each test specimen are given in Table 3.9. The time-dependent development of cracking, including the crack spacing and crack width, was measured in each specimen throughout the test. The measured elastic modulus and compressive strength of the concrete at the age of ﬁrst loading were Ec = 22,820 MPa and fc = 18.3 MPa, whilst the measured creep coefﬁcient and shrinkage strain associated with the 400-day period of sustained loading were ϕ(t, τ ) = 1.71 and εsh = −0.000825. Two identical specimens ‘a’ and ‘b’ were constructed for each combination of parameters as indicated in Table 3.9, with the ‘a’ specimens loaded more heavily than the ‘b’ specimens. The ‘a’ specimens were subjected to a constant sustained load sufﬁcient to cause a maximum moment at mid-span of between 40 and 50 per cent of the calculated ultimate moment and the ‘b’ specimens were subjected to a constant sustained mid-span moment of between 25 and 40 per cent of the calculated ultimate moment.

250 mm

400 mm 300 mm sb

sb

cb

cb

130 mm

Ast

Ast cs

cs (a) Beams

(b) Slabs

Figure 3.7 Cross-sections of test specimens (Ref. 35).

Table 3.9 Details of the test specimens (Ref. 35) Beam No. of db Ast cs sb cb bars (mm) (mm2 ) (mm) (mm) (mm)

Slab No. of db Ast cs sb cb bars (mm) (mm2 ) (mm) (mm) (mm)

B1-a B1-b B2-a B2-b B3-a B3-b

S1-a S1-b S2-a S2-b S3-a S3-b

2 2 2 2 3 3

16 16 16 16 16 16

400 400 400 400 600 600

40 40 25 25 25 25

40 40 25 25 25 25

154 154 184 184 92 92

2 2 3 3 4 4

12 12 12 12 12 12

226 226 339 339 452 452

25 25 25 25 25 25

40 40 40 40 40 40

308 308 154 154 103 103

The loads on all specimens were sufﬁcient to cause primary cracks to develop in the region of maximum moment at ﬁrst loading. In Table 3.10, the sustained in-service moment at mid-span, Msus , is presented, together with the stress in the tensile steel at mid-span, σst1 , due to Msus (calculated on the basis of a

Design for serviceability

81

fully cracked section); the calculated ultimate ﬂexural strength, Mu (assuming a characteristic yield stress of the reinforcing steel of 500 MPa); the ratio Msus /Mu ; and the cracking moment, Mcr (calculated assuming a tensile strength of concrete of 0.6 fc (t), where fc (t) is the measured compressive strength at the time of loading in MPa).

Table 3.10 Moments and steel stresses in the test specimens (Ref. 35) Beam Mcr Msus σst1 Mu Msus /Mu (kNm) (kNm) (MPa) (kNm) (%)

Slab Mcr Msus σst1 Mu Msus /Mu (kNm) (kNm) (MPa) (kNm) (%)

B1-a B1-b B2-a B2-b B3-a B3-b

S1-a S1-b S2-a S2-b S3-a S3-b

14.0 14.0 13.1 13.1 13.7 13.7

24.9 17.0 24.8 16.8 34.6 20.8

227 155 226 153 214 129

56.2 56.2 56.2 56.2 81.5 81.5

44.3 30.2 44.1 29.8 42.4 25.5

4.65 4.65 4.75 4.75 4.86 4.86

6.81 5.28 9.87 6.81 11.4 8.34

252 195 247 171 216 159

13.9 13.9 20.3 20.3 26.4 26.4

49.0 38.0 48.6 33.6 43.0 31.6

At ﬁrst loading, a regular pattern of primary cracks developed in each test specimen. With time, the cracks gradually increased in width and additional cracks developed between some of the primary cracks. Thus, the average crack spacing reduced with time. The ratio of ﬁnal to initial crack spacing ranged from 0.57 to 0.85, with an average value of 0.70. Crack widths increased rapidly in the ﬁrst few weeks after loading, but the rate of increase slowed signiﬁcantly after about 2 months. For all specimens, there was little change in the maximum crack width after about 200 days under load. Typical calculations for the maximum crack width are provided here for Beam B2-a. Beam B2-a: Typical maximum crack width calculations are provided here for Beam B2-a, with b = 250 mm, D = 333 mm, d = 300 mm, Ast = 400 mm2 , Ec = 22820 MPa, n = Es /Ec = 8.76. A cracked section analysis gives kd = 78.8 mm and Icr = 212 × 106 mm4 . The applied moment at mid-span is Msus = 24.8 kN and the stress in the tensile steel on the cracked section is: σst1 =

nMsus (d − kd) 8.76 × 24.8 × 106 × (300 − 78.8) = = 226 MPa Icr 212 × 106

Gergely and Lutz: For B2-a, c1 = 33 mm, A = (250 × 66)/2 = 8250 mm2 and from Eq. 3.35: w = 0.011 ×

333 − 78.8 × 226 × (33 × 8250)0.33 = 0.178 mm 300 − 78.8

82 Design for serviceability Frosch: For B2-a, the bar spacing is sb = 184 mm and from Eq. 3.36: 226 333 − 78.8 w = 2× × × 332 + (184/2)2 = 0.254 mm 200,000 300 − 78.8 Eurocode 2 (1992): For B2-a, the additional parameters required for the Eurocode 2 (1992) approach are: β = 1.7; β1 = 1.0; β2 = 0.5 for sustained loading; fctm = 2.08 MPa; σsr = (Mcr /Ms ) σst1 = 96.8 MPa; k1 = 0.8; k2 = 0.5; Ac.eff = 2.5 × 33 × 250 = 20,625 mm2 ; ρeff = 400/20,625 = 0.0194; and srm = 50 + 0.25 × 0.8 × 0.5 × 16/0.0194 = 132 mm. From Eq. 3.37:

226 96.8 2 w = 1.7 × 132 × = 0.232 mm 1 − 1.0 × 0.5 × 200,000 226 Eurocode 2 (2004): For B2-a, the additional parameters required for the Eurocode 2 (2004) approach are: c = 25 mm; fct,eff = 2.08 MPa; and from Eq. 3.41, sr,max = 3.4×25+0.425× 0.8 × 0.5 × 16/0.0194 = 225 mm. Now σst1 /Es = 0.00113 and from Eq. 3.40: εsm − εcm = 0.00113 − 0.4 × 2.08 × (1 + 8.76 × 0.0194)/(200,000 × 0.0194) = 0.000881. From Eq. 3.39: w = 225 × 0.000881 = 0.198 mm Calculated versus measured maximum crack width: For this specimen, all four calculation methods signiﬁcantly underestimate the measured maximum ﬁnal crack width of 0.36 mm. The measured and calculated maximum ﬁnal crack widths for all 12 beam and slab specimens are compared in Table 3.11. The mean of the ratios of predicted to measured crack widths and the coefﬁcient of variation for each calculation method are also provided for both the beam and the slab specimens. For the beam specimens, all four calculation methods signiﬁcantly underestimate the measured maximum crack width. The Eurocode 2 (1992) approach has the lowest coefﬁcient of variation. None of the calculation methods adequately accounts for the very signiﬁcant time-dependent increase in crack width due to drying shrinkage. In fact, the crack width predicted by each of the methods is independent of the level of drying shrinkage or the creep coefﬁcient. For the slab specimens, the Gergely and Lutz method (Eq. 3.35) provides a reasonable estimate of maximum crack width for this set of test data. Both Eurocode 2 approaches again have the lowest coefﬁcients of variation, but underestimate the measured test data. The expression proposed by Frosch (Eq. 3.36) tends to overestimate the measured maximum crack width, particularly when the bar spacing is wide (such as in specimens S1-a and S1-b).

Design for serviceability

83

Table 3.11 Comparison of measured and predicted maximum ﬁnal crack widths (mm) Specimen Measured Gergely and Lutz (mm) (Eq. 3.35)

Frosch (Eq. 3.36)

Eurocode 2 1992 (Eq. 3.37)

Eurocode 2 2004 (Eq. 3.39)

Predicted Predicted/ Predicted Predicted/ Predicted Predicted/ Predicted Predicted/ (mm) Measured (mm) Measured (mm) Measured (mm) Measured B1-a B1-b B2-a B2-b B3-a B3-b

0.38 0.18 0.36 0.18 0.28 0.13

0.242 0.165 0.178 0.121 0.149 0.089

Mean Coefﬁcient of variation (%) S1-a S1-b S2-a S2-b S3-a S3-b

0.25 0.20 0.23 0.18 0.20 0.15

0.254 0.197 0.221 0.153 0.179 0.131

Mean Coefﬁcient of variation (%)

0.638 0.919 0.494 0.670 0.531 0.688

0.251 0.171 0.254 0.172 0.141 0.085

0.661 0.952 0.707 0.957 0.503 0.651

0.242 0.143 0.232 0.138 0.179 0.097

0.637 0.796 0.644 0.769 0.638 0.747

0.250 0.146 0.198 0.116 0.157 0.082

0.658 0.811 0.551 0.645 0.562 0.634

0.657

0.739

0.705

0.644

22.8

24.5

10.4

14.5

1.015 0.984 0.962 0.848 0.895 0.873

0.520 0.403 0.274 0.189 0.176 0.129

2.081 2.016 1.192 1.051 0.881 0.859

0.257 0.176 0.211 0.132 0.160 0.111

1.029 0.878 0.917 0.735 0.801 0.738

0.218 0.150 0.184 0.113 0.142 0.096

0.872 0.749 0.800 0.629 0.708 0.639

0.930

1.346

0.849

0.733

7.2

41.4

13.5

12.8

3.7.3 Tension chord model for ﬂexural cracking in reinforced concrete A model for predicting the maximum ﬁnal crack width (w∗ ) in reinforced concrete ﬂexural members based on the tension chord model of Marti et al. (Ref. 32) was recently proposed (Ref. 34). A modiﬁed version of that model is presented here and has been shown to provide good agreement with the measured ﬁnal spacing and width of cracks in reinforced concrete beams and slabs under sustained loads. The notation associated with the model is shown in Fig. 3.8. Consider a segment of a singly reinforced beam of rectangular section subjected to an in-service bending moment, Ms , greater than the cracking moment, Mcr . The spacing between the primary cracks is s, as shown in Fig. 3.8a. A typical cross-section between the cracks is shown in Fig. 3.8b and a cross-section at a primary crack is shown in Fig. 3.8c. The cracked beam is idealised as a compression chord of depth kd and width b and a cracked tension chord consisting of the tensile reinforcement of area Ast surrounded by an area of tensile concrete (Act ) as shown in Fig. 3.8d. The centroids of Ast and Act are assumed to coincide at a depth d below the top ﬁbre of the section. For the sections containing a primary crack (Fig. 3.8c), Act = 0 and the depth of the compressive zone, kd, and the second moment of area about the centroidal axis (Icr ) may be determined from a cracked section analysis using modular ratio theory (Eqs 3.14 and 3.17). Away from the crack, the area of the concrete in the tension chord of Fig. 3.8d (Act ) is assumed to carry a uniform tensile stress (σct ) that develops due to the bond stress (τb ) that exists between the tensile steel and the surrounding concrete.

84 Design for serviceability b

b kd d

Ms h

(1−k)d Ast

Ast s

Primary crack

(a) Beam elevation

(c) Cracked section

(b) Uncracked section

b C

C

kd d

Cracked tension chord Ts + Tc

T s

Ast Act

(d) Idealised compression and tension chord model

Figure 3.8 Cracked reinforced concrete beam and idealised tension chord model (Ref. 34).

For the tension chord, the area of concrete between the cracks, Act , may be taken as: Act = 0.5(D − kd)b∗

(3.45)

where b∗ is the width of the section at the level of the centroid of the tensile steel (i.e. at the depth d) but not greater than the number of bars in the tension zone multiplied by 12db . At each crack, the concrete carries no tension and the tensile steel stress is σst1 = T/Ast , where: T=

nMs (d − kd) Ast Icr

(3.46)

As the distance z from the crack in the direction of the tension chord increases, the stress in the steel reduces due to the bond shear stress τb between the steel and the surrounding tensile concrete. For reinforced concrete under service loads, where σst1 is less than the yield stress fy , Marti et al. (Ref. 33) assumed a rigid-plastic bond shear stress-slip relationship, with τb = 2.0fct at all values of slip, where fct is the direct tensile strength of the concrete. To account for the reduction in bond stress with time due to tensile creep and shrinkage, Gilbert (Ref. 34) took the bond stress to be τb = 2.0fct for short-term calculations and τb = 1.0fct when the ﬁnal long-term crack width was to be determined. Experimental observations (Refs 35 and 36) indicate that τb reduces as the stress in the reinforcement increases and, consequently, the tensile stresses in the concrete between the cracks reduces (i.e. tension stiffening reduces with increasing steel stress). In reality, the magnitude of τb is affected by many factors, including steel

Design for serviceability

85

stress, concrete cover, bar spacing, transverse reinforcement (stirrups), lateral pressure, compaction of the concrete, size of bar deformations, tensile creep and shrinkage. It is recommended here that in situations where the concrete cover and the clear spacing between the bars are greater than the bar diameter, the bond stress τb may be taken as: τb = λ1 λ2 λ3 fct

(3.47)

where λ1 accounts for the load duration with λ1 = 1.0 for short-term calculations and λ1 = 0.7 for long-term calculations; λ2 is a factor that accounts for the reduction in bond stress as the steel stress σst1 (in MPa) increases and is given by (Ref. 36): ˙ st1 ≥ 0.0 λ2 = 1.66˙ − 0.003σ

(3.48)

and λ3 is a factor that accounts for the very signiﬁcant increase in bond stress that has been observed in laboratory tests for small diameter bars (Ref. 35) and may be taken as: λ3 = 7.0 − 0.3db ≥ 2.0 (db in mm)

(3.49)

An elevation of the tension chord is shown in Fig. 3.9a and the stress variations in the concrete and steel in the tension chord are illustrated in Figs 3.9b and 3.9c, respectively. Following the approach of Marti et al. (Ref. 33), the concrete and steel tensile stresses in Figs 3.9b and 3.9c, where 0 < z ≤ s/2, may be expressed as: σstz =

T 4τ z − b Ast db

(3.50a)

tb T Crack

s/2

Crack

s/2

(a) Elevation of tension chord between cracks z

sc2

(b) Tensile concrete stress sst1

sst1 sst2

(c) Tensile steel stress

Figure 3.9 Tension chord – actions and stresses (Ref. 33).

86 Design for serviceability and σcz =

4τb ρtc z db

(3.50b)

where ρtc is the reinforcement ratio of the tension chord (= Ast /Act ) and db is the reinforcing bar diameter. Mid-way between the cracks, at z = s/2, the stresses are: σst2 =

T 2τ s − b As db

(3.51a)

σc2 =

2τb ρtc s db

(3.51b)

and

The maximum crack spacing immediately after loading, s = smax , occurs when σc2 = fct , and from Eq. 3.51b: smax =

fct db 2τb ρtc

(3.52)

with λ1 = 1.0 in Eq. 3.47. If the spacing between two adjacent cracks just exceeds smax , the concrete stress mid-way between the cracks will exceed fct and another crack will form between the two existing cracks. It follows that the minimum crack spacing is half the maximum value, that is, smin = smax /2. The instantaneous crack width (wi )tc in the ﬁctitious tension chord is the difference between the elongation of the tensile steel over the length s and the elongation of the concrete between the cracks and is given by: (wi )tc =

s T τ s − b (1 + nρtc ) Es Ast db

(3.53)

Depending on the dimensions of the cross-section and the concrete cover, the instantaneous crack width at the bottom concrete surface of the beam or slab, (wi )sofﬁt , may be different from that given by Eq. 3.53 for the tension chord and may be obtained from:

kcover s T τb s (wi )sofﬁt = kcover (wi )av = − (1 + nρtc ) Es Ast db

(3.54)

where kcover is a term to account for the dependence of crack width on the clear concrete cover c and may be taken as: kcover =

D − kd d − kd

5c (D − kd) − 2db

0.3 (3.55)

Design for serviceability

87

Under sustained load, additional cracks occur between widely spaced cracks (usually when 0.67smax < s ≤ smax ). The additional cracks are due to the combined effect of tensile creep rupture and shrinkage. As a consequence, the number of cracks increases and the maximum crack spacing reduces with time. The ﬁnal maximum crack spacing s∗ is only about two-thirds of that given by Eq. 3.52, but the ﬁnal minimum crack spacing remains about half of the value given by Eq. 3.52. As previously mentioned, experimental observations indicate that τb decreases with time, probably as a result of shrinkage-induced slip and tensile creep. Hence, the stress in the tensile concrete between the cracks gradually reduces. Furthermore, although creep and shrinkage will cause a small increase in the resultant tensile force T in the real beam and a slight reduction in the internal lever arm, this effect is relatively small and is ignored in the tension chord model presented here. The ﬁnal crack width is the elongation of the steel over the distance between the cracks minus the extension of the concrete caused by σcz plus the shortening of the concrete between the cracks due to shrinkage. For a ﬁnal maximum crack spacing of s∗ , the ﬁnal maximum crack width at the member sofﬁt is:

kcover s∗ T τb s∗ (w )sofﬁt = − (1 + ne ρtc ) − εsh Es Es Ast db ∗

(3.56)

where εsh is the shrinkage strain in the tensile concrete (and is a negative value); ne = Es /Ee = the effective modular ratio; Ee is the effective modulus given by Ee = Ec /(1 + ϕ(t, τ )); Ec and Es are the elastic moduli of the concrete and steel respectively; and ϕ(t, τ ) is the creep coefﬁcient of the concrete. A good estimate of the ﬁnal maximum crack width is given by Eq. 3.56, where s∗ is the maximum crack spacing after all time-dependent cracking has taken place, that is, s∗ = 0.67smax , and smax is given by Eq. 3.52. By rearranging Eq. 3.56, the steel stress on a cracked section corresponding to a particular maximum ﬁnal crack width (w∗ ) is given by: fst =

w ∗ Es τb s∗ + (1 + ne ρtc ) + εsh Es s∗ kcover db

(3.57)

By substituting τb (from Eq. 3.47) and s∗ = 0.67smax into Eq. 3.57 and by selecting a maximum desired crack width in a particular structure, w∗ , the maximum permissible tensile steel stress can be determined.

Example 3.6 The maximum ﬁnal crack widths determined using Eq. 3.56 are compared with the measured maximum ﬁnal crack widths for the 12 prismatic, oneway singly reinforced concrete specimens (six beams and six slabs) tested by Gilbert and Nejadi (Ref. 35). The specimens were described in Example 3.5 and their cross-sections are shown in Fig. 3.7 and details provided in Tables 3.9 and 3.10. Typical maximum crack width calculations are provided here for Beam B2-a.

88 Design for serviceability

Beam B2-a Relevant dimensions and properties are: b = 250 mm, D = 333 mm, d = 300 mm, Ast = 400 mm2 , Ec = 22,820 MPa, n = Es /Ec = 8.76, ϕ(t, τ ) = 1.71, εsh = −0.000825, Ee = 8420 MPa and ne = 23.8. A cracked section analysis gives kd = 78.8 mm and Icr = 212 × 106 mm4 . From Eq. 3.45, the area of concrete in the tension chord is Act = 0.5 × (333 − 78.8) × 250 = 31,780 mm2 and the reinforcement ratio of the tension chord ρtc = Ast /Act = 0.0126. When Ms = 24.8 kNm, the tensile force in the steel on the cracked section is Eq. 3.46: T=

8.76 × 24.8 × 106 (300 − 78.8) × 400 = 90.6 kN 212 × 106

and σst1 =

T = 226 MPa Ast

For short-term calculations, λ1 = 1.0 and, from Eqs 3.48 and 3.49, λ2 = 1.6 6˙ − 0.003˙ × 226 = 0.91 and λ3 = 7.0 − 0.3 × 16 = 2.2. With fct = 0.6 f c (t) = 2.57 MPa, the instantaneous bond stress is obtained from Eq. 3.47 as τb = 1.0 × 0.91 × 2.2 × 2.57 = 5.15 MPa and the maximum crack spacing immediately after loading is given by Eq. 3.52: smax =

2.57 × 16 = 317 mm 2 × 5.15 × 0.0126

For the calculation of the maximum ﬁnal crack width, the maximum crack spacing s∗ is taken as 2/3 of the instantaneous value and therefore s∗ = 2/3 × 317 = 211 mm. From Eq. 3.47, for long-term calculations, τb = 0.7 × 0.91 × 2.2 × 2.57 = 3.60 MPa and, from Eq. 3.55, kcover = 0.967. The maximum ﬁnal (long-term) crack width at the sofﬁt of the beam specimen B2-a is obtained from Eq. 3.56:

0.967 × 211 90,600 3.60 × 211 (w )sofﬁt = − (1 + 23.8 × 0.0126) 200,000 400 16 ∗

− (−0.000825) × 200,000 = 0.337 mm The measured maximum ﬁnal crack width on this specimen after 400 days under load was 0.36 mm. The measured and calculated maximum ﬁnal crack widths for all 12 test specimens are compared in Table 3.12. The mean of the ratios of predicted to measured crack widths for the six beam specimens is 1.059, with a coefﬁcient of variation of 22.8 per cent while for the six slab specimens the mean is 0.945, with a coefﬁcient of variation of 17.7 per cent. The agreement between the calculated and measured maximum ﬁnal crack width for this set of test data is good.

Design for serviceability Table 3.12 Comparison of measured and predicted maximum ﬁnal crack widths (mm) Specimen

B1-a

B1-b

B2-a

B2-b

B3-a

B3-b

S1-a

S1-b

S2-a

S2-b

S3-a

S3-b

Measured, wmax 0.38 0.18 0.36 0.18 0.28 0.13 0.25 0.20 0.23 0.18 0.20 0.15 Predicted, (w∗ )sofﬁt 0.425 0.262 0.337 0.207 0.212 0.122 0.287 0.196 0.258 0.155 0.162 0.111 1.119 1.457 0.935 1.149 0.758 0.936 1.148 0.981 1.123 0.863 0.812 0.742 (w∗ )sofﬁt /wmax

Example 3.7 A 150 mm thick simply-supported one-way slab located inside a building is to be considered. With appropriate regard for durability, the concrete strength is selected to be fc = 32 MPa and the cover to the tensile reinforcement is 20 mm. The ﬁnal shrinkage strain is taken to be εsh = −0.0006. Other relevant material properties are Ec = 28,600 MPa; n = Es /Ec = 7.0; ϕ(t, τ ) = 2.5; fct = 2.04 MPa and Es = 200 GPa. The effective modulus is therefore Ee = Ec /(1 + ϕ(t, τ )) = 8170 MPa and the effective modular ratio ne = Es /Ee = 24.5. The tensile face of the slab is to be exposed and the maximum ﬁnal crack width is to be limited to w∗ = 0.3 mm. After completing the design for strength and deﬂection control, the required minimum area of tensile steel is 650 mm2 /m. Under the full service loads, the maximum in-service sustained moment at mid-span is 20.0 kNm/m. The bar diameter and bar spacing must be determined so that the requirements for crack control are also satisﬁed.

Case 1 – Use 10 mm bars at 120 mm centres Ast = 655 mm2 /m at d = 125 mm and, referring to Figs 3.5 and 3.8, an elastic analysis of the cracked section gives kd = 29.6 mm and Icr = 50.3×106 mm4 . The maximum in-service tensile steel stress on the fully-cracked section at mid-span is calculated using Eq. 3.46 as σst1 = T/As = 265 MPa. The area of concrete in the tension chord is Act = 60,200 mm2 (Eq. 3.45) and the reinforcement ratio of the tension chord is ρtc = As /Act = 0.0109. From Eqs 3.48 and 3.49, λ2 = 0.78 and λ3 = 4.0 and from Eq. 3.47, τb = 6.39 MPa for short-term calculations (λ1 = 1.0) and τb = 4.47 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing s∗ is obtained using Eq. 3.52 as s∗ = 0.67smax = 97.6 mm and Eq. 3.55 gives kcover = 1.26. The maximum permissible steel stress required for crack control is obtained from Eq. 3.57: fst =

0.3 × 200,000 4.47 × 97.6 + (1 + 24.5 × 0.0109) 97.6 × 1.26 10 + (−0.0006 × 200,000) = 422 MPa

The actual stress at the crack σst = 265 MPa is much less than fst = 422 MPa and, therefore, cracking is easily controlled.

89

90 Design for serviceability

Case 2 – Use 12 mm bars at 170 mm centres As = 665 mm2 /m at d = 124 mm and, for this section, kd = 29.6 mm and Icr = 50.1 × 106 mm4 . The maximum in-service tensile steel stress on the fullycracked section at mid-span is σst1 = T/As = 264 MPa. The area of concrete in the tension chord is Act = 50,980 mm2 and ρtc = As /Act = 0.0130. Now λ2 = 0.79 and λ3 = 3.4 and τb = 5.47 MPa for shortterm calculations (λ1 = 1.0) and τb = 3.83 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing is s∗ = 114 mm and from Eq. 3.55, kcover = 1.29. The maximum permissible steel stress required for crack control is obtained from Eq. 3.57 as fst = 335 MPa – which is also signiﬁcantly greater than the actual maximum stress at the crack σst = 264 MPa. Therefore, the ﬁnal maximum crack width will be less than the maximum permissible value of 0.3 mm.

Case 3 – Use 16 mm bars at 300 mm centres As = 670 mm2 /m at d = 122 mm and, for this section, kd = 29.4 mm and Icr = 48.6 × 106 mm4 . The maximum in-service tensile steel stress on the fullycracked section at mid-span is σst1 = T/As = 266 MPa. The area of concrete in the tension chord is Act = 38,580 mm2 and ρtc = As /Act = 0.0174. Now λ2 = 0.78 and λ3 = 2.2 and τb = 3.50 MPa for short-term calculations (λ1 = 1.0) and τb = 2.45 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing is s∗ = 179 mm and from Eq. 3.55, kcover = 1.35. The maximum permissible steel stress required for crack control is fst = 167 MPa (from Eq. 3.57), which is much less than the actual steel stress due to the sustained moment of σst = 266 MPa. Therefore, crack control is not adequate and the maximum ﬁnal crack width will exceed 0.3 mm.

Simpliﬁed approaches – case 3 The deemed-to-comply crack control provisions of Eurocode 2 (2004) are in reasonable agreement with the above calculations, while the ACI 318-08 (Ref. 4) provisions are not. Considering ﬁrst the Eurocode 2 provisions, for case 3 above, the area of tensile steel provided exceeds the minimum steel area given by Eq. 3.42 and Table 3.7 suggests that, for a steel stress of σst1 = 266 MPa, if the maximum crack width is to be limited to 0.3 mm, the maximum bar diameter for crack control is 12 mm. Considering the ACI 318-08 requirement for Case 3, the area of tensile reinforcement exceeds the minimum value Ast.min given by Eq. 3.43, and with a steel stress of σst1 = 266 MPa, the maximum bar spacing permitted by Eq. 3.44 is 315 mm. With the bar spacing of 300 mm, Case 3 satisﬁes the requirements for crack control in ACI 318-08. The maximum crack widths predicted by the Gergely and Lutz expression (Eq. 3.35) and the two Eurocode 2 equations (Eqs 3.37 and 3.39) for case 3 are 0.284 mm, 0.304 mm and 0.244 mm, respectively. These indicate that the

Design for serviceability

91

maximum ﬁnal crack width will be less than (or in the case of Eurocode 2 (1992) only just greater than) the design crack width w∗ = 0.3 mm. In a structural design situation, all three approaches suggest that case 3 is acceptable. By contrast, the maximum crack width given by the equation proposed by Frosch (Eq. 3.36) is 0.528 mm, indicating that case 3 will lead to excessively wide cracks.

3.7.4 Model for direct tension cracking in restrained reinforced concrete Consider the fully restrained member shown in Fig. 3.10a (Refs 37 and 38). As the concrete shrinks, the restraining force N(t) gradually increases until the ﬁrst crack occurs when N(t) = Ac fct (t) (usually within a week of the commencement of shrinkage). At ﬁrst cracking, the restraining force reduces to Ncr , and the concrete stress away from the crack is less than the tensile strength of the concrete fct . The concrete on either side of the crack shortens elastically and the crack opens to a width w(t) that depends on the area of reinforcement (see Fig. 3.10b). At the crack, the steel carries the entire force Ncr and the stress in the concrete is clearly zero. In the region adjacent to the crack, the concrete and steel stresses vary considerably and the bond stress at the steel-concrete interface is high. At some distance so on each side of the crack, the concrete and steel stresses are no longer inﬂuenced directly by the presence of the crack, as shown in Figs 3.10c and 3.10d. Referring to Fig. 3.10, numerical values of Ncr , σc1 , σs1 , and σs2 can be obtained from (Ref. 37): Ncr =

nρfct Ac C1 + nρ(1 + C1 )

(3.58a)

σc1 =

Ncr (1 + C1 ) Ac

(3.58b)

σs1 = −C1 σs2 σs2 =

Ncr As

(3.58c) (3.58d)

where n is the modular ratio (Es /Ec ); ρ is the reinforcement ratio (As /Ac ); fct is the direct tensile strength of the concrete at ﬁrst cracking; and C1 =

2so 3L − 2so

(3.59)

The distance so in which stresses vary on either side of a crack depends on those factors that affect the bond stress at the steel concrete interface and include the reinforcement quantity, the bar diameter db and the surface characteristics of the bar. In Ref. 37 so was taken to be: so =

db 10ρ

(3.60)

92 Design for serviceability As = area of reinforcing steel Ac = area of concrete N(t)

N(t) (=Ac fct)

L

(a) Just prior to first cracking w Ncr

Ncr

L

(b) Just after first cracking so w so

sc1 Region 1

sc1 Region 2

Region 1

(c) Concrete stress just after first cracking ss2

ss1

so so w

ss1

(d) Steel stress just after first cracking

Figure 3.10 First cracking in a restrained direct tension member (Ref. 37).

This expression was used earlier by Favre et al. (Ref. 39) and others for a member containing deformed bars or welded wire mesh. Recent experimental results (Ref. 40) suggest that shrinkage causes a deterioration in bond at the steel-concrete interface and a gradual increase in so with time. For calculations at ﬁrst cracking (Eqs 3.58 and 3.59), so may be taken from Eq. 3.60, and for ﬁnal or long-term calculations, the value of so from Eq. 3.60 should be multiplied by 1.33 (Ref. 38) (i.e. (s∗o = 1.33 so ). The ﬁnal number of cracks and the ﬁnal average crack width depend on the length of the member, the quantity and distribution of reinforcement, the quality of bond between the concrete and steel, the amount of shrinkage and the concrete properties. In Fig. 3.11a, a portion of a restrained direct tension member is shown after all shrinkage has taken place and the ﬁnal crack pattern is established. The average concrete and steel stresses caused by shrinkage are illustrated in Figs 3.11bbreak and 3.11c. In many practical situations, the supports of a reinforced concrete member that provide the restraint to shrinkage are not immovable, but instead are adjacent parts of the structure that are themselves prone to shrinkage and other movements. If the supports of the restrained member in Fig. 3.10a suffer a relative movement u with time (in the direction of the length L), such that the ﬁnal length of the member is (L + u), the ﬁnal restraining force N(∞) changes and this affects both the crack

Design for serviceability w

w

93

w

s

s

(a) Portion of a restrained member after all cracking w

w

s*o s*o

s*o

w s*o

s*o

s *c1 Region 2

Region 1

s*o

s *c1 Region 2

Region 1

Region 2

(b) Concrete stress after all shrinkage cracking

s *s2

s *s2

s *s1

s *s2

s *s1

(c) Steel stress after all shrinkage cracking

Figure 3.11 Final concrete and steel stresses after direct tension cracking (Ref. 37).

spacing and the crack width. If u increases, N(∞) increases and so too does the number and width of the cracks. By enforcing the requirements of compatibility and equilibrium, expressions for the ﬁnal average crack spacing (s) and ﬁnal crack width (w) in a restrained member can be derived (Ref. 37). For a member containing m cracks and providing the reinforcing steel has not yielded, equating the overall elongation of the steel reinforcement to u gives:

∗ ∗ σ ∗ − σs1 σs1 2 ∗ L + m s2 (3.61) so + w = u Es Es 3 and, as w is much less than so , rearranging gives: ∗ σs1 =

−2 s∗o m ∗ 3 u Es σs2 + ∗ 3L − 2so m 3L − 2s∗o m

(3.62)

At each crack: ∗ σs2 = N(∞)/As

(3.63)

In Region 1 in Fig. 3.11, where the distance away from each crack exceeds s∗o (with taken as 1.33 times the value given by Eq. 3.60), the concrete stress history is shown diagrammatically in Fig. 3.12. The concrete tensile stress increases gradually with time as shrinkage progresses and approaches the direct tensile strength of the concrete fct . When cracking occurs elsewhere in the member, the tensile stress in the s∗o

94 Design for serviceability Concrete stress

fct sav sc1

s *c1

Time First cracking

Figure 3.12 Concrete stress history in uncracked Region 1 (Ref. 37).

uncracked regions drops suddenly as shown. Although the concrete stress history is continually changing, the average concrete stress at any time after the start of drying, σav , is between σc1 and fct , as shown in Fig. 3.12, and may be taken as the average of σc1 and fct (Ref. 37). The ﬁnal creep strain in Region 1 may be approximated by: εc∗ =

σav ∗ ϕ (τd ) Ec

(3.64)

where ϕ ∗ (τd ) is the ﬁnal creep coefﬁcient (at time inﬁnity) and τd is the age of the concrete when drying ﬁrst commenced. The ﬁnal concrete strain in Region 1 is the sum of the elastic, creep, and shrinkage components and may be approximated as: ∗ ε1∗ = εe + εc∗ + εsh =

σav σav ∗ ∗ + ϕ (τd ) + εsh Ec Ec

(3.65)

and the magnitude of the ﬁnal creep coefﬁcient ϕ ∗ (τd ) is usually between 2 and 4, depending on the age at the commencement of drying and the quality of the concrete. Eq. 3.65 may be expressed as: ε1∗ =

σav ∗ + εsh Ee

(3.66)

Ec ). 1 + φ ∗ (τd ) In Region 1, at any distance from a crack greater than so , equilibrium requires that the sum of the force in the concrete and the force in the steel is equal to N(∞). That is:

where Ee is the ﬁnal effective modulus for concrete (Ee =

∗ ∗ ∗ σc1 Ac + σs1 As = N(∞) or σc1 =

∗A N(∞) − σs1 s Ac

(3.67)

The compatibility requirement is that the ﬁnal concrete and steel strains are identical ∗ = ε ∗ ). Using Eq. 3.66, this becomes: (εs1 1 ∗ σs1 σav ∗ = + εsh Ee Es

(3.68)

Design for serviceability

95

Substituting Eqs 3.62 and 3.63 into Eq. 3.68 and rearranging gives: N(∞) =

3As Es u (3L − 2s∗o m)ne As ∗ Ee ) − (σav + εsh 2s∗o m 2s∗o m

(3.69)

With the restraining force N(∞) and the steel stress in Region 1 obtained from Eqs 3.69 and 3.62, respectively, the ﬁnal concrete stress in Region 1 is ∗ σc1 =

∗A N(∞) − σs1 s Ac

(3.70)

∗ ≤ f , where The number of cracks m is the lowest integer value of m for which σc1 ct the direct tensile strength fct should be taken as the mean 28-day value. The ﬁnal average crack spacing is s = L/m. The overall shortening of the concrete is an estimate of the sum of the crack widths. The ﬁnal concrete strain at any point in Region 1 of Fig. 3.11 is given by Eq. 3.66, and in Region 2, the ﬁnal concrete strain is:

ε2∗ =

∗ fnσc1 ∗ + εsh Ee

(3.71)

where fn varies between zero at a crack and unity at so from a crack. If a parabolic variation of stress is assumed in Region 2, the following expression for the average crack width w is obtained by integrating the concrete strain over the length of the member:

∗

σ 2 ∗ w = − c1 s − s∗o + εsh s (3.72) Ee 3 The preceding analysis is valid provided the assumption of linear-elastic behaviour in the steel is valid, that is, provided the steel has not yielded.

Example 3.8 The 140 mm thick slab of length 4 m shown in Fig. 3.13 is to be considered. The slab is rigidly held in position at each end support and, except for shrinkage, is unloaded. The slab is symmetrically reinforced with 12 mm diameter bars at 250 mm centres near both the top and bottom surfaces. Hence, As = 900 mm2 /m and ρ = As /Ac = 0.00643. The average ﬁnal spacing between the restrained shrinkage cracks and the average ﬁnal crack width are to be determined. D = 140 mm

L=4m

Figure 3.13 Slab of Example 3.8.

The material properties are: fc = 25 MPa; fct = 2.5 MPa; Ec = 25000 MPa; n = Es /Ec = 8.0; ϕ(t, τ ) = 3.0; E∗e = Ec /(1+ϕ ∗ (τ )) = 6250 MPa; ∗ ne = Es /E∗e = 32; and ∗ = −0.0007. εsh

96 Design for serviceability From Eqs 3.60 and 3.59: 12 = 187 mm and 10 × 0.00643 2 × 187 C1 = = 0.0321. 3 × 4000 − 2 × 187 so =

From Eqs 3.58a and b: Ncr =

8 × 0.00643 × 2.5 × 140,000 = 211 kN; 0.0321 + 8 × 0.00643 × (1 + 0.0321)

σc1 =

211,000 × (1 + 0.0321) = 1.55 MPa; 140,000

and therefore σav =

σc1 + fct = 2.02 MPa. 2

For ﬁnal shrinkage calculations: s∗o = 1.33 × 187 = 248 mm. The tabulation below shows the ﬁnal restraining force and concrete and steel stresses for different numbers of cracks: Number of cracks, m

N(∞) from Eq. 3.69 (kN)

∗ from σs1 Eq. 3.62 (MPa)

∗ from σs2 Eq. 3.63 (MPa)

∗ from σc1 Eq. 3.70 (MPa)

3 4 5 6

477 341 259 205

−75.1 −75.1 −75.1 −75.1

530 379 288 227

3.89 2.92 2.33 1.94

After the ﬁfth crack forms, the ﬁnal concrete stress is less than the tensile strength of concrete and the ﬁnal crack spacing is therefore about s = L/m = 800 mm. The ﬁnal crack width is estimated from Eq. 3.72:

2.33 2 w=− (800 − × 248) + (−0.0007 × 800) = 0.32 mm 6250 3

3.8 References 1. Sbarounis, J.A. (1984). Multi-storey ﬂat plate buildings – measured and computer one-year deﬂections. Concrete International, 6(8), 31–35. 2. Jokinen, E.P. and Scanlon, A. (1985). Field Measured Two-way Slab Deﬂections. CSCE Annual Conference, Saskatoon, Canada. 3. Gilbert, R.I. (1999). The risk and responsibility of structural engineers – A case study of a structural failure. International Congress – Creating with Concrete, University of Dundee, Scotland, Sept. Concrete Durability and Repair Technology, Thomas Telford, pp 773–783.

Design for serviceability

97

4. American Concrete Institute (2008), Building Code Requirements for Structural Concrete, ACI 318-08, Detroit. 5. British Standards Institution (1992). Eurocode 2: Design of Concrete Structures – Part 1: General rules and rules for buildings – DD ENV 1992-1-1:1992. European Committee for Standardization, Brussels. 6. British Standards Institution (2004). Eurocode 2: Design of Concrete Structures – part 1-1: General rules and rules for buildings – BS EN 1992-1-1:2004. European Committee for Standardization, Brussels. 7. Standards Australia (2009). Australian Standard for Concrete Structures, AS3600-2009. Sydney. 8. Standards Australia (2002). Structural design actions – Permanent, imposed and other actions AS/NZS 1170.1. Amendment 1: 2005, Amendment 2: 2009 (Australian/New Zealand Standards). 9. Standards Australia (2004). Bridge Design Part 2: Design Loads AS5100.2-2004. Sydney. 10. National Research Council of Canada (2005). National Building Code of Canada. Ottawa, Ontario. 11. British Standards Institution (1996). BS 6399: Part 1 – Loading for Buildings – Code of Practice for Dead and Imposed Loads. London. 12. American Association of State Highway and Transportation Ofﬁcials (2002). Standard Speciﬁcations for Highway Bridges AASHTO HB-17, Washington, DC. 13. American Society of Civil Engineers (2005). ASCE Standard ASCE 7-05 - Minimum Design Loads for Buildings and Other Structures. Reston, Virginia. 14. Standards Australia (2002). Structural design actions – Wind actions AS/NZS 1170.2. Amendment 1: 2005 (Australian/New Zealand Standards). 15. British Standards Institution (1997). BS 6399: Part 2 – Loading for Buildings – Code of Practice for Wind Loads. London. 16. Structural Engineers Association of California (2009). SEAOC Blue Book – Seismic Design Recommendations. Seismology Committee, Sacramento, CA. 17. Branson, D.E. (1965). Instantaneous and time-dependent deﬂections of simple and continuous reinforced concrete beams. HPR Report No. 7. Part 1. Alabama Highway Dept. Bureau of Public Roads, Alabama. 18. Gilbert, R.I. (2007). Tension stiffening in lightly reinforced concrete slabs. Journal of Structural Engineering, ASCE, 133(6), 899–903. 19. Irwin, A.W. (1978). Human response to dynamic motion of structures. The Structural Engineer, 56A(9). 20. Wilford, M. and Yound, P. (2006). A Design Guide for Footfall induced Vibrations of Structures. The Concrete Centre, Camberley, UK. 21. Mayer, H. and Rüsch, H. (1967). Building Damage Caused by Deﬂection of Reinforced Concrete Building Components. Technical Translation 1412, National Research Council Ottawa, Canada (Deutscher Auschuss für Stahlbeton, Heft 193, Berlin, West Germany, 1967). 22. Rangan, B.V. (1982). Control of beam deﬂections by allowable span-depth ratios. ACI Journal, 79(5), 372–377. 23. Gilbert, R.I. (1985). Deﬂection control of slabs using allowable span to depth ratios. ACI Journal, 82(1), 67–72. 24. The Concrete Society (2005). Deﬂections in concrete slabs and beams. Technical Report No. 58. 25. Bischoff, P.H. (2005). Reevaluation of deﬂection prediction for concrete beams reinforced with steel and FRP bars. Journal of Structural Engineering, ASCE, 131(5), 752–767. 26. Gilbert, R.I. (1999). Deﬂection calculations for reinforced concrete structures – why we sometimes get it wrong. ACI Structural Journal, 96(6), 1027–1032.

98 Design for serviceability 27. Patrick, M. (2009). Beam deﬂection by simpliﬁed calculation: including effect of compressive reinforcement in formula for σcs in draft AS3600. BD-002 Committee Document. 28. Gilbert R.I. (2003). Deﬂection by simpliﬁed calculation in AS3600-2001 – on the determination of fcs . Australian Journal of Structural Engineering, Engineers Australia, 5(1), 61–71. 29. Gilbert, R.I. (2008). Instantaneous and time-dependent deﬂection of reinforced concrete ﬂexural members. Concrete Forum – Journal of the Concrete Institute of Australia, 1(1), 7–17. 30. Gilbert, R.I. (2001). Deﬂection calculation and control – Australian code amendments and improvements. In ACI International SP 203, Code Provisions for Deﬂection Control in Concrete Structures, Chapter 4, American Concrete Institute. Editors E.G. Nawy and A. Scanlon, Detroit, 45–78. 31. Gergely, P. and Lutz, L.A. (1968). Maximum crack width in reinforced concrete ﬂexural members. In Causes, Mechanism, and Control of Cracking in Concrete, SP-20, American Concrete Institute, Farmington Hills, MI, 1–17. 32. Frosch, R.J. (1999). Another look at cracking and crack control in reinforced concrete. ACI Structural Journal, 96(3), 437–442. 33. Marti, P., Alvarez, M., Kaufmann, W. and Sigrist, V. (1998). Tension chord model for structural concrete. Structural Engineering International, 4/98, 287–298. 34. Gilbert, R.I. (2008). Control of ﬂexural cracking in reinforced concrete. ACI Structural Journal, 105(3), 301–307. 35. Gilbert, R.I. and Nejadi, S. (2004). An Experimental Study of Flexural Cracking in Reinforced Concrete Members under Sustained Loads. UNICIV Report No. R-435, School of Civil and Environmental Engineering, University of New South Wales, Sydney, Australia. 36. Wu, H.Q. and Gilbert, R.I. (2009). Modelling short-term tension stiffening in reinforced concrete prisms using a continuum-based ﬁnite element model. Engineering Structures, 31(10), 2380–2391. 37. Gilbert, R.I. (1992). Shrinkage cracking in fully-restrained concrete members. ACI Structural Journal, 89(2), 141–149. 38. Nejadi, S. and Gilbert, R.I. (2004). Shrinkage cracking and crack control in restrained reinforced concrete members. ACI Structural Journal, 101(6), 840–845. 39. Favre, R. et al. (1983). Fissuration et Deformations. Manual du Comite Euro-International du Beton (CEB), Ecole Polytechnique Federale de Lausanne, Switzerland. 40. Nejadi, S. and Gilbert, R.I. (2004). Shrinkage Cracking in Restrained Reinforced Concrete Members. UNICIV Report No. R-433, School of Civil and Environmental Engineering, The University of New South Wales, Sydney, Australia.

4

Uncracked sections Axial loading

4.1 Preamble In the previous chapter, simpliﬁed methods were presented for the determination of deﬂection and crack widths. While often suitable for design purposes, the simpliﬁed methods approximate structural deformation at service loads without necessarily providing an insight into the time-dependent behaviour of the structure. In situations where accurate and reliable estimates of the effects of creep and shrinkage are required, the simpliﬁed methods of Chapter 3 may not be adequate. More reﬁned methods are available that realistically model the time-dependent deformation of concrete structures and also enable the calculation of the redistribution of stresses between the concrete and the reinforcement and the redistribution of internal actions in statically indeterminate members. Reﬁned methods for the time analysis of cross-sections are introduced in this chapter and illustrated using the simple example of a symmetrically reinforced cross-section subjected to a constant sustained axial compressive load. The time analysis of a concrete structure involves the determination of strains, stresses, curvatures and deﬂections at critical points and at critical times during the life of the structure. Often a structural designer is most interested in the ﬁnal deformation and the ﬁnal internal actions at time inﬁnity after the effects of creep and shrinkage have taken place, i.e. the long-term behaviour. The creep and shrinkage characteristics of concrete are highly variable and are never known exactly. In addition, the methods for the time analysis of concrete structures are plagued by simplifying assumptions and approximations. Accurate numerical predictions of time-dependent behaviour are therefore not possible. However, it is possible, and indeed necessary, to establish upper and lower limits to the ﬁnal stresses and deformations in order to determine whether or not time effects are critical in any particular situation and, if required, to adjust the design in order to reduce undesirable long-term deformations. If the concrete stress σc (τ0 ) at a point in a structure, ﬁrst applied at age τ0 , remains constant with time, each of the concrete strain components may be calculated readily as follows: ε (t) = εe (t) + εcr (t) + εsh (t) =

σc (τ0 ) σc (τ0 ) + ϕ(t, τ0 ) + εsh (t) Ec (τ0 ) Ec (τ0 )

(4.1)

Numerical values of ϕ(t, τ0 ) and εsh (t) may be obtained from the models discussed in Sections 2.1.4 and 2.1.5, and the calculation of time-dependent structural behaviour is relatively straightforward.

100 Uncracked sections If the concrete stress at a point varies with time, the determination of the creep strain becomes more involved. In reinforced concrete structures, even under constant sustained loads, stresses are rarely constant and Eq. 4.1 can no longer be used to predict deformation accurately. The stress history and the effects of ageing must be included. In this chapter, several methods for the time analysis of cross-sections are discussed and applied to a simple practical problem. The mathematical description of each procedure is followed by a discussion of its strengths and weaknesses, and its advantages and disadvantages. To illustrate each procedure, the analysis of a symmetrically reinforced concrete column section under a constant axial compressive load is presented and numerical results obtained using each procedure are compared.

4.2 The effective modulus method 4.2.1 Formulation The simplest and oldest technique for including creep in structural analysis is Faber’s effective modulus method (EMM) (Ref. 1). In Section 1.2.4, the instantaneous and creep components of strain were combined and a reduced or effective modulus for concrete, Ee (t, τ0 ), was deﬁned in Eqs 1.11 and 1.12. In Section 1.2.5, the integraltype creep law was presented in Eq. 1.17 to describe the time-dependent deformation of a continuously varying stress history. In the EMM, Eq. 1.17 is approximated by assuming that the stress-dependent deformations are produced only by a sustained stress equal to the ﬁnal value of the stress history, that is: t ε(t) = τ0

=

1 + ϕ (t, τ ) 1 + ϕ (t, τ0 ) dσc (τ ) + εsh (t) ≈ σc (t) + εsh (t) Ec (τ ) Ec (τ0 )

σc (t) + εsh (t) Ee (t, τ0 )

(4.2)

where Ee (t, τ0 ) is the effective modulus for concrete deﬁned in Eq. 1.12 (which for convenience is repeated here) as: Ee (t,τ0 ) =

Ec (τ0 ) 1 + ϕ(t,τ0 )

(4.3)

Creep is treated as a delayed elastic strain and is taken into account simply by reducing the elastic modulus of concrete with time. A time analysis using the effective modulus method is nothing more than an elastic analysis in which Ee (t, τ0 ) is used instead of Ec (τ0 ). Shrinkage may be included in this elastic time analysis in a similar way as a sudden temperature change in the concrete would be included in a short-term elastic analysis. According to the EMM, the creep strain at time t (in Eq. 4.2) depends only on the current stress in the concrete σc (t) and is therefore independent of the previous stress history. This, of course, is not the case. The ageing of the concrete has been ignored. For an increasing stress history, the EMM overestimates creep, while for a decreasing

Uncracked sections 101 stress history, creep is underestimated. If the stress is entirely removed, the creep strains disappear. The EMM therefore predicts complete creep recovery, which is not correct. Eq. 4.2 is valid only when the concrete stress is constant in time. In such cases, the EMM gives excellent results. Good results are also obtained if the concrete is old when ﬁrst loaded and the effect of ageing is not great. Despite its shortcomings, the EMM is the simplest of all of the methods for the time analysis of concrete structures and its simplicity recommends it, particularly under the conditions mentioned above. In many practical problems, the method is sufﬁciently accurate for design purposes. However, many practical situations involve rapidly changing stress histories in young concrete. In such cases, the EMM may be unsuitable and potentially misleading, and a more sophisticated method of analysis is required. 4.2.2 Example application (EMM) Consider the short, axially-loaded, symmetrically reinforced column shown in Fig. 4.1. The column is subjected to a constant, sustained axial force P as shown. Creep and shrinkage cause a gradually decreasing stress history in the concrete similar to that shown in Fig. 1.15. The redistribution of internal forces due to the gradual development of creep and shrinkage strains is to be examined and the time-dependent stresses and strains in both the concrete and the steel are to be calculated using the EMM. The problem is solved by enforcing the three basic requirements of any time analysis: namely, equilibrium of forces, compatibility of strains and satisfaction of the constitutive relationships of the concrete and the steel. The external compressive load P is applied at time τ0 and is resisted by the internal forces in the concrete and steel Nc (t) and Ns (t), where at any time t after loading Nc (t) = σc (t)Ac and Ns (t) = σs (t)As . Equilibrium requires that the sum of the internal forces at time t equals the external load, that is: P = Nc (t) + Ns (t) = σc (t)Ac + σs (t)As

P

(4.4)

P P = constant

Ac L Nc(t) Ns(t)

(a) Elevation

As

(b) Section

Figure 4.1 Axially-loaded short column.

102 Uncracked sections Compatibility requires that the total concrete strain ε(t) and the steel strain εs (t) are identical at all times: ε(t) = εs (t)

(4.5)

The concrete constitutive relationship used in the EMM is given by Eq. 4.2 and the steel is assumed to be linear and elastic, with modulus Es . Therefore, at any time t: ε(t) =

σc (t) + εsh (t) Ee (t, τ0 )

(4.6a)

and σs (t) Es

εs (t) =

(4.6b)

Re-arranging Eqs 4.6 in terms of σc (t) and σs (t) gives: σc (t) = ε(t)Ee (t, τ0 ) − εsh (t)Ee (t, τ0 )

(4.7a)

σs (t) = εs (t)Es

(4.7b)

and

Inserting these equations into the equilibrium equation (Eq. 4.4) and enforcing compatibility (Eq. 4.5) yields: P = Ee (t, τ0 )ε(t)Ac − Ee (t, τ0 )εsh (t)Ac + ε(t)Es As

(4.8)

which represents the governing equation of the problem. Solving Eq. 4.8 for the unknown total concrete strain ε(t) gives: ε(t) = =

P Ac Ee (t, τ0 )εsh (t) + Ac Ee (t, τ0 ) + As Es Ac Ee (t, τ0 ) + As Es P ε (t) + sh Ac Ee (t, τ0 )(1 + ne ρ) 1 + ne ρ

(4.9)

where ne = the effective modular ratio = Es /Ee (t, τ0 ) and ρ = the reinforcement ratio = As /Ac . By substituting Eq. 4.9 into Eq. 4.7a, the concrete stress at time t is obtained: σc (t) =

P Es ρ εsh (t) − Ac (1 + ne ρ) 1 + ne ρ

(4.10)

The steel strain εs (t) is identical to the total concrete strain ε(t) (Eq. 4.5) and therefore the steel stress may be obtained by substituting Eq. 4.9 into Eq. 4.7b: σs (t) =

ne P Es εsh (t) + Ac (1 + ne ρ) 1 + ne ρ

(4.11a)

Uncracked sections 103 The steel stress may also be obtained from the equilibrium equation (Eq. 4.4): σs (t) =

P − σc (t)Ac As

(4.11b)

The elastic component of concrete strain at time t is usually taken to be εe (t) = σc (t)/Ec (τ0 ) and the creep strain is therefore εcr (t) = ε(t) − εe (t) − εsh (t).

Example 4.1 Consider the short, symmetrically reinforced column shown in Fig. 4.1. The column is subjected to a constant sustained axial force P = −1000 kN ﬁrst applied at age τ0 = 14 days. The cross-sectional areas of the concrete and the steel reinforcement are Ac = 90,000 mm2 and As = 1800 mm2 , respectively, and the reinforcement ratio is therefore ρ = As /Ac = 0.02. The column is located in a temperate environment and shrinkage is assumed to commence at the age of ﬁrst loading. The mean in-situ compressive strength of concrete at the time of ﬁrst loading is taken to be fcmi (τ0 ) = 28 MPa and the characteristic 28-day compressive strength is fc = 40 MPa. The elastic modulus of concrete at ﬁrst loading is Ec (τ0 ) = 26.7 GPa and the elastic modulus of steel is Es = 200 GPa. The creep coefﬁcient is obtained from Eq. 2.3 and shrinkage strain is obtained ∗ = −510×10−6 . from Eq. 2.6, with ﬁnal (long-term) values: ϕ ∗ (τ0 ) = 2.39 and εsh The variations of the creep coefﬁcient and shrinkage with time are given in the following table and shown in Fig. 4.2. For illustrative purposes it has been assumed that shrinkage begins at the time of loading. (t − τ0 ) in days

0

10

30

70

200

500

10,000

ϕ(t, τ0 ) εsh (t − τ0 ) × 10−6

0 0

0.53 −142

0.98 −246

1.38 −325

1.83 −407

2.10 −456

2.39 −510

Creep coefficient

2.5 2 1.5 1 0.5 0 0

200

400

600

Time, t (days)

800

1000

Shrinkage strain (× −10−6)

The redistribution of internal forces due to the gradual development of creep and shrinkage strains is to be examined and the time-dependent changes in stresses and strains in both the concrete and the steel are to be calculated. Sample calculations are provided below. 600 500 400 300 200 100 0 0

200

400

600

800

1000

Time, t (days)

Figure 4.2 Creep coefﬁcient and shrinkage strain versus time curves for Example 4.1.

104 Uncracked sections

At ﬁrst loading τ0 , (t − τ0 ) = 0: ϕ(t, τ0 ) = 0 and εsh (t − τ0 ) = 0. With Ee (t, τ0 ) = Ec (τ0 ) = 26.7 GPa; and ne = n = Es /Ec (τ0 ) = 7.48. Eq. 4.9: Eq. 4.5:

ε(τ0 ) =

−1000 × 103 + 0 = −361 × 10−6 ; 90,000 × 26,700 × (1 + 7.48 × 0.02)

εs (τ0 ) = −361 × 10−6 ;

Eq. 4.7a:

σc (τ0 ) = −361 × 10−6 × 26,700 − 0 = −9.67 MPa;

Eq. 4.7b:

σs (τ0 ) = −361 × 10−6 × 200,000 = −72.3 MPa.

The stresses in the concrete and steel could have also been calculated directly from Eqs 4.10 and 4.11: Eq. 4.10:

σc (τ0 ) =

−1000 × 103 − 0 = −9.67 MPa; 90,000(1 + 7.48 × 0.02)

Eq. 4.11b:

σs (τ0 ) =

−1000 × 103 + 9.67 × 90,000 = −72.3 MPa. 1800

With the creep and shrinkage components of the concrete strain both equal to zero at ﬁrst loading, the concrete strain ε(τ0 ) is entirely made up of the elastic or instantaneous component of strain εe (τ0 ).

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + ϕ(t, τ0 )) = 17.48 GPa; and ne = Es /Ee (t, τ0 ) = 11.44; and Eq. 4.9:

ε(t) =

−1000 × 103 −142 × 10−6 + 90,000 × 17,480 × (1 + 11.44 × 0.02) 1 + 11.44 × 0.02

= −633 × 10−6 ; Eq. 4.5: Eq. 4.7a:

εs (t) = −633 × 10−6 ; σc (t) = −633 × 10−6 × 17,480 − (−142 × 10−6 ) × 17,480 = −8.58 MPa;

Eq. 4.7b:

σs (t) = −633 × 10−6 × 200,000 = −126.6 MPa.

The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −321 × 10−6 ; the shrinkage component of strain is εsh (t) = −142 × 10−6 ; and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −170 × 10−6 .

Uncracked sections 105 The results of the analyses at ﬁrst loading and throughout the period of sustained loading are provided in the following table. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) −9.67 −8.58 −7.82 −7.23 −6.66 −6.35 −6.02

0 10 30 70 200 500 10,000

Steel stress σs (t) (MPa) −72.3 −127 −165 −194 −222 −238 −255

Total Elastic Creep Shrinkage strain concrete strain strain ε(t) strain εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −633 −824 −969 −1112 −1191 −1273

−361 −321 −292 −270 −249 −237 −225

0 −170 −285 −374 −456 −497 −538

0 −142 −246 −325 −407 −456 −510

4.3 The principle of superposition – step-by-step method (SSM) 4.3.1 Formulation The principle of superposition and its applicability for the determination of strains in concrete was discussed in Section 1.2.5. The creep strain produced by a stress increment applied at any time τi is assumed to be unaffected by any other stress increment applied either earlier or later. The superposition integral for the total concrete strain at any time t due to a time-varying stress history (Eq. 1.17) cannot be solved in closed form unless simplifying assumptions are made, such as the parallel creep curve assumption illustrated subsequently in Fig. 4.10. In the step-by-step method (SSM), a solution technique is employed using the incremental form of the superposition equation (Eq. 1.16). The period of sustained stress is divided into k time intervals as shown in Fig. 4.3, with the age at ﬁrst loading designated τ0 and the end of the period of sustained stress designated τk . Consider the time-varying stress history shown in Fig. 4.4. The actual stress history is approximated by a step-wise variation of stress, with an increment of stress σc (τj ) applied at the end of each time interval, as shown. For this decreasing stress history, if the initial stress σc (τ0 ) is compressive, the stress increments σc (τj ) applied at the end of each time interval are tensile. The stress is assumed to remain constant during Concrete pour t0 t 1

t2

tj

tk-1

First loading

tk

Time, t

End of time period

Figure 4.3 Time discretisation.

106 Uncracked sections Stress sc(t0)

sc(t) Dsc(tj)

j-th time interval, Dtj

t 0 t1 t 2

tj−1

tj

tk Time

Figure 4.4 Time-varying stress history – SSM.

each time interval. The greater the number of time intervals, the more accurate is the ﬁnal prediction. Various formulations of the SSM are available in the literature (for example, Refs 2–5), all of which give similar answers provided the time intervals are suitably small. For a particular time interval τk − τ0 , the time discretisation should be such that an approximately equal portion of the creep coefﬁcient ϕ(τk , τ0 ) develops during each time step. A convenient and effective time discretisation based on a geometrical progression is given by: (τk − τ0 ) τk k 1/(k−1) τj = τ0 + τk k τj−1 − τ0 τ1 = τ0 +

(4.12a) (4.12b)

where τ0 and τk deﬁne the beginning and end of the time period to be discretised; k represents the number of time intervals; and j = 2, 3, . . ., k. The SSM is perfectly general and can be used to predict behaviour due to any stress or strain history using any desired creep and shrinkage curves. Using the integral in the integral-type creep law (Eq. 1.17): t ε(t) = J (t, τ0 )σc (τ0 ) +

J (t, τ )dσc (τ ) + εsh (t)

τ0+

and the total concrete strain at the end of the j-th time period (t = τj ) may be approximated by:

ε(τj ) = J (τj , τ0 )σc (τ0 ) +

j J τj , τi σc (τi ) + εsh (τj )

(4.13a)

i=1

where J(τj , τi ) represents the creep (compliance) function calculated at time τj related to a unit stress applied at time τi , while σc (τi ) is calculated as σc (τi )−σc (τi−1 ) and depicts the stress variation that occurs between times τi−1 and τi . A better approximation is

Uncracked sections 107 obtained if the average creep function associated with the time step τi and τi−1 is used within the summation in Eq. 4.13a, that is: j J τj , τi + J τj , τi−1 σc (τi ) + εsh (τj ) ε(τj ) = J (τj , τ0 )σc (τ0 ) + 2

(4.13b)

i=1

Eq. 4.13a approximates the integral-type creep law by means of the so-called rectangular rule, while Eq. 4.13b represents the trapezoidal rule. Both approximations tend towards the same result as the number of time steps increases. Simplifying the notation, Eqs 4.13a and 4.13b become, respectively: εj − εsh,j = Jj,0 σc,0 +

j

Jj,i σc,i

(4.13c)

i=1

and εj − εsh,j = Jj,0 σc,0 +

j Jj,i + Jj,i−1

2

i=1

σc,i

(4.13d)

where εj = ε(τj ); εsh,j = εsh (τj ); Jj,0 = J (τj , τ0 ); σc,0 = σc (τ0 ); Jj,i = J τj , τi ; σc,i = σc (τi ) and σc (τi ) = σc,i − σc,i−1 . Eqs 4.13a and b can be expressed in terms of creep coefﬁcients as follows: j

ε(τj ) =

1 + ϕ (τj , τi ) 1 + ϕ (τj , τ0 ) σc (τ0 ) + σc (τi ) + εsh (τj ) Ec (τ0 ) Ec (τi )

(4.14a)

i=1

and

j 1+ϕ (τj ,τ0 ) 1 1+ϕ (τj ,τi ) 1+ϕ (τj ,τi−1 ) σc (τ0 )+ + σc (τi )+εsh (τj ) ε(τj ) = Ec (τ0 ) 2 Ec (τi ) Ec (τi−1 ) i=1

(4.14b) Simplifying the notation gives: j

εj − εsh,j =

1 + ϕj,i 1 + ϕj,0 σc,0 + σc,i Ec,0 Ec,i

(4.14c)

i=1

and j

1 1 + ϕj,0 σc,0 + εj − εsh,j = Ec,0 2 i=1

1 + ϕj,i−1 1 + ϕj,i + Ec,i Ec,i−1

σc,i

where ϕj,0 = ϕ(τj , τ0 ), ϕj,i = ϕ (τj , τi ), Ec,0 = Ec (τ0 ) and Ec,i = Ec (τi ).

(4.14d)

108 Uncracked sections As Eqs 4.14 indicate, a large amount of input data is required for the SSM. For each time step, Ec (τi ) and ϕ(τj , τi ) must be speciﬁed and the previous stress history must be stored throughout the analysis. However, the SSM is not subject to many of the simplifying assumptions contained in other methods of analysis and generally leads to reliable results. For most practical problems, satisfactory results are obtained using as few as 6–10 time intervals. For illustrative purposes, Eqs 4.13a and 4.14a are used in the following. The axially loaded, symmetrically reinforced column shown in Fig. 4.1, and analysed in Section 4.2.2, is re-analysed here using the SSM. Time is discretised into a preselected number of time intervals. Two approaches will be considered: (i) Approach 1 obtains the solution by calculating the change in concrete stress that occurs at the end of each time step; and (ii) Approach 2 expresses the governing system of equations in terms of the concrete stress at the time considered. Both approaches are in fact identical and differ only in the manipulation of the governing equations. 4.3.2 Example application (SSM) – Approach 1 In Approach 1, Eq. 4.14a is used to calculate the change in stress at the end of each time step. For the continuously varying stress history shown in Fig. 4.4, the stress increment, σc (τi ), is assumed to be applied at the end of the i-th time interval, as shown. The increments of instantaneous plus creep strain caused by σc (τi ) are calculated at the end of each time interval using the appropriate elastic modulus and creep coefﬁcient (Ec (τi ) and ϕ(τj , τi ), respectively). The total strain at the end of each time interval is obtained by superposition of the strain increments caused by stress changes in all previous time intervals and by shrinkage. 4.3.2.1 At ﬁrst loading (t = τ0 ) Following the approach outlined in Section 4.2.2 for the EMM, the instantaneous stresses and strains at τ0 immediately after the application of the axial force P, and before any creep and shrinkage has occurred, are obtained using Eqs 4.5–4.11 and are given by: ε(τ0 ) =

P ; εs (τ0 ) = ε(τ0 );σc (τ0 ) = ε(τ0 )Ec (τ0 ); and σs (τ0 ) = εs (τ0 )Es Ac Ec (τ0 )(1+n0 ρ)

where n0 = Es /Ec (τ0 ) = the modular ratio at time τ0 and ρ = As /Ac = the reinforcement ratio. The analysis at each subsequent time step is outlined in the following. 4.3.2.2 At the end of the j-th time step (i.e. t = τj ) The stress in the concrete at the end of the j-th time step is: σc (τj ) = σc (τj−1 ) + σc (τj )

(4.15)

Uncracked sections 109 where σc (τj−1 ) is known as it has been calculated at the previous time step and σc (τj ) is the unknown stress increment at τj . The equilibrium and compatibility equations are:

σc (τj−1 ) + σc (τj ) Ac + σs (τj ) As = P

(4.16)

and ε(τj ) = εs (τj )

(4.17)

The stress–strain relationships for the concrete and the steel at time τj are: j

ε(τj ) =

1 + ϕ (τj , τi ) 1 + ϕ (τj , τ0 ) σc (τ0 ) + σc (τi ) + εsh (τj ) Ec (τ0 ) Ec (τi )

(4.18a)

i=1

and εs (τj ) =

σs (τj ) Es

(4.18b)

Rearranging Eqs 4.18 in terms of stresses at time τj gives: j−1 Ec (τj ) σc (τi ) σc (τ0 ) − Ec (τj ) − Ec (τj )εsh (τj ) σc τj = Ec (τj )ε(τj ) − Ee (τj , τ0 ) Ee (τj , τi ) i=1

(4.19a) and σs τj = Es εs (τj )

(4.19b)

where Ee (τj , τi ) is the effective modulus of concrete at time τj associated with a stress increment ﬁrst applied at time τi and is given by: Ee (τj , τi ) =

Ec (τi ) 1 + ϕ (τj , τi )

(4.20)

By substituting Eqs 4.19 and 4.17 into Eq. 4.16 and simplifying, the unknown strain, ε(τk ), is readily determined as: ⎤ ⎡ j−1 σc (τj−1 ) ne,j,0 σc (τ0 ) ne,j,i σc (τi ) 1 P ⎣ + + εsh (τj )⎦ − + ε(τj ) = 1 + nj ρ Ac Ec (τj ) Ec (τj ) Es Es i=1

(4.21)

110 Uncracked sections where nj = Es /Ec (τj ) = the modular ratio at time τj ; ne,j,0 = Es /Ee (τj , τ0 ) and ne,j,i = Es /Ee (τj , τi ) are the effective modular ratios; and ρ = the reinforcement ratio = As /Ac . The steel strain εs (τj ) is found using Eq. 4.17 and is identical to the total concrete strain ε(τj ). The concrete stress increment is obtained from Eq. 4.19a: ⎡ σc (τj ) =

1 ⎣ P − σc (τj−1 ) − ne,j,0 ρσc (τ0 ) − 1 + nj ρ Ac

j−1

⎤ ne,j,i ρσc (τi ) − εsh (τj )Es ρ ⎦

i=1

(4.22) With σ (τj ) calculated from Eq. 4.22, the concrete stress at τj is obtained from Eq. 4.15. The steel stress σs (τj ) is determined from Eq. 4.19b. Alternatively, σs (τj ) could also be calculated from the equilibrium equation (Eq. 4.16). From the strain calculated at time instant τj (ε(τj ) = εs (τj )), the axial deformation or axial shortening of the column can be readily calculated. For the column of length, L, shown in Fig. 4.1, the axial shortening of the column at time, τj , due to the applied load, P, and shrinkage is designated eL (τj ) and given by: eL (τj ) = Lε(τj )

(4.23)

The approach is useful in the determination of time-dependent axial shortening in the columns and walls of multi-storey buildings where differential shortening may be an important design consideration.

Example 4.2 The symmetrically reinforced column analysed in Example 4.1 (refer Fig. 4.1) is to be re-analysed here using the SSM. As in the previous example, the column is subjected to an axial load P = −1000 kN ﬁrst applied at age τ0 = 14 days and then held constant. The properties of the column cross-section are: Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; and Es = 200 GPa. In this example, the six time intervals speciﬁed in the following table are considered for illustrative purposes. A signiﬁcant amount of input data is required; speciﬁcally, a different creep coefﬁcient and elastic modulus for each concrete stress increment applied at the end of each time interval. The following table contains the input data necessary to obtain the concrete and steel stresses and strains at the end of each time interval. The concrete properties are obtained from the material modelling procedures outlined in Chapter 2, that is, Ec (τj ) from Eqs 2.2a and 2.2c, ϕ(τj , τi ) from Eq. 2.3 and εsh (τj ) from Eq. 2.6. The concrete is mixed with high early strength cement. As in Example 4.1, shrinkage is taken to begin at the time of ﬁrst loading.

Uncracked sections 111 j

0

1

2

3

4

5

6

τj (days)

14

24

44

84

214

514

10,014

t − τj (days)

0

10

30

70

200

500

10,000

ϕ(τj , τ0 ) ϕ(τj , τ1 ) ϕ(τj , τ2 ) ϕ(τj , τ3 ) ϕ(τj , τ4 ) ϕ(τj , τ5 )

0

0.53 0

0.98 0.72 0

1.38 1.18 0.90 0

1.83 1.63 1.44 1.22 0

2.10 1.89 1.69 1.51 1.26 0

2.39 2.15 1.94 1.75 1.54 1.38

Ec (τj ) (MPa)

26,700

27,900

28,900

29,700

30,500

31,000

31,700

εsh (τj ) × 10−6

0

−142

−246

−325

−407

−456

−510

Note that the shrinkage strains and the creep coefﬁcients associated with the age at ﬁrst loading, τ0 , are the same as those adopted previously in Example 4.1 using the EMM. The family of creep coefﬁcient versus the logarithm of time curves is shown in Fig. 4.5. 3

Creep coefficient

2.5 2 1.5 1 0.5

j(t,t0)

0

14

j(t,t2) j(t,t1)

24

44

10

j(t,t3) j(t,t4)

84 100

214

j(t,t5)

514 1000

10,000

Time (days) (log scale)

Figure 4.5 Creep coefﬁcient versus log time curves for Example 4.2.

At ﬁrst loading (τ0 ): As in Example 4.1, with Ec (τ0 ) = Ee (τ0 , τ0 ) = 26.7 GPa and n0 = Es /Ec (τ0 ) = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε(τ0 ) = −361 × 10−6 ; εs (τ0 ) = −361 × 10−6 ; σc (τ0 ) = −9.67 MPa and σs (τ0 ) = −72.3 MPa.

At time instant τ1 = 24 days (time step 1 from τ0 to τ1 ): For time interval, j = 1: Ec (τ0 ) = 26.7 GPa; Ec (τ1 ) = 27.9 GPa; n1 = Es /Ec (τ1 ) = 7.17; ϕ(τ1 , τ0 ) = 0.53; Ee (τ1 , τ0 ) = Ec (τ0 )/(1 + ϕ(τ1 , τ0 )) = 17.48 GPa; ne,1,0 = Es /Ee (τ1 , τ0 ) = 11.44; and εsh (τ1 ) = −142 × 10−6 .

112 Uncracked sections From Eq. 4.22:

1 −1000 × 103 σc (τ1 ) = + 9.67 + 11.44 × 0.02 × 9.67 1 + 7.17 × 0.02 90,000 + 142 × 10−6 × 200,000 × 0.02 = 1.17 MPa

The concrete stress at τ1 is therefore σc (τ1 ) = σc (τ0 ) + σc (τ1 ) = −9.67 + 1.17 = −8.50 MPa −1000 × 103 + 8.50 × 90,000 = −131 MPa 1800 Eq. 4.18b and Eq. 4.17 give: and from Eq. 4.16: σs (τ1 ) =

εs (τ1 ) =

−131 = −653 × 10−6 200,000

ε(τ1 ) = −653 × 10−6 At time τ1 , the elastic component of the concrete strain is εe (τ1 ) = σc (τ0 )/Ec (τ0 )+ σ (τ1 )/Ec (τ1 ) = −319 × 10−6 ; the shrinkage component of strain is εsh (τ1 ) = −142 × 10−6 ; and therefore the creep component of strain is εcr (τ1 ) = ε(τ1 ) − εe (τ1 ) − εsh (τ1 ) = −192 × 10−6 .

At time instant τ2 = 44 days (time step 2 from τ1 to τ2 ): Time interval, j= 2: Ec (τ0 ) = 26.7 GPa; Ec (τ1 ) = 27.9 GPa; Ec (τ2 ) = 28.9 GPa; n2 = Es /Ec (τ2 ) = 6.92; ϕ(τ2 , τ0 ) = 0.98; Ee (τ2 , τ0 ) = Ec (τ0 )/(1 + ϕ(τ2 , τ0 )) = 13.53 GPa; ne,2,0 = Es /Ee (τ2 , τ0 ) = 14.78; ϕ(τ2 , τ1 ) = 0.72; Ee (τ2 , τ1 ) = Ec (τ1 )/(1 + ϕ(τ2 , τ1 )) = 16.25 GPa; ne,2,1 = Es /Ee (τ2 , τ1 ) = 12.31; εsh (τ2 ) = −246 × 10−6 . Eq. 4.22: 1 −1000×103 σ (τ2 ) = +8.50+14.78×0.02× 1+6.92×0.02 90,000 ×9.67 −12.31×0.02×1.17 +246×10

−6

×200,000×0.02

= 0.83 MPa The concrete stress at τ2 is therefore: σc (τ2 ) = σc (τ1 ) + σc (τ2 ) = −8.50 + 0.83 = −7.67 MPa

Uncracked sections 113 and from Eq. 4.16, the steel stress is: σs (τ2 ) =

−1000 × 103 + 7.67 × 90,000 = −172 MPa 1800

The steel strain is obtained from Eq. 4.18b and the total concrete strain from Eq. 4.17: εs (τ2 ) =

−172 = −860 × 10−6 200,000

and ε (τ2 ) = −860 × 10−6 At time τ2 , the elastic component of concrete strain is: εe (τ2 ) = σc (τ0 )/Ec (τ0 ) + σc (τ1 )/Ec (τ1 ) + σc (τ2 )/Ec (τ2 ) = −291 × 10−6 ; the shrinkage component is εsh (τ2 ) = −246 × 10−6 ; and therefore the creep component of strain is: εcr (τ2 ) = ε(τ2 ) − εe (τ2 ) − εsh (τ2 ) = −323 × 10−6 .

At subsequent time instants Similarly, the stress and strain components at the end of each subsequent time step are calculated and the results are tabulated below. Instant Time τj Concrete Concrete Steel Total Elastic Creep Shrinkage j (days) stress stress stress strain strain strain strain increment σc (τj ) σs (τj ) ε(τj ) εe (τj ) εcr (τj ) εsh (τj ) σc (τj ) (MPa) (MPa) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) (MPa) 0 1 2 3 4 5 6

14 24 44 84 214 514 10,014

– 1.17 0.83 0.63 0.65 0.34 0.41

−9.67 −8.50 −7.67 −7.04 −6.39 −6.05 −5.64

−72.3 −131 −172 −204 −236 −253 −273

−361 −653 −860 −1018 −1180 −1264 −1367

−361 −319 −291 −269 −248 −237 −225

0 −192 −323 −424 −525 −571 −632

0 −142 −246 −325 −407 −456 −510

The effect of increasing the number of time steps on the accuracy of the predictions using the SSM is illustrated below. In the following table, the results of further analyses are presented in which the time discretisation proposed in Eqs 4.12 has been adopted. Either 6 or 18 time steps have been considered between τ0 and each of the previously considered time instants (τk in the ﬁrst

114 Uncracked sections column of the table below). The results provided on each line of the table have been produced by separate time analyses using the SSM. Time τk (days)

14 24 44 84 214 514 10,014

No of time steps used

Concrete stress σc (τk ) (MPa)

Steel stress (MPa)

Total strain ε(τk ) (×10−6 )

Elastic strain εe (τk ) (×10−6 )

Creep strain εcr (τk ) (×10−6 )

Shrinkage strain εsh (τk ) (×10−6 )

1 6 (18) 6 (18) 6 (18) 6 (18) 6 (18) 6 (18)

−9.67 −8.54 (−8.55) −7.68 (−7.72) −7.02 (−7.09) −6.36 (−6.46) −6.00 (−6.10) −5.65 (−5.71)

−72.3 −129 (−128) −171 (−169) −205 (−201) −238 (−233) −255 (−251) −273 (−270)

−361 −644 (−641) −857 (−847) −1023 (−1006) −1188 (−1164) −1277 (−1253) −1366 (−1349)

−361 −320 (−320) −291 (−292) −269 (−270) −247 (−249) −236 (−238) −225 (−226)

0 −182 (−179) −320 (−309) −430 (−411) −534 (−508) −586 (−559) −631 (−613)

0 −142 (−142) −246 (−246) −325 (−325) −407 (−407) −456 (−456) −510 (−510)

Based on these results, increasing the number of time steps by a factor of three has produced changes in the ﬁnal total strain and in the ﬁnal concrete and steel stresses of less than 2 per cent. Considering the uncertainty associated with the estimates of the concrete properties, there is little to be gained, from a practical point of view, by considering more than about 6–10 time steps in most situations. The axial shortening of the column is calculated using Eq. 4.23. If the overall length of the column is 4000 mm, the column shortening at ﬁrst loading and after 10,000 days are eL (τ0 = 14) = 1.44 mm and eL (τ18 = 10,014) = 5.40 mm, respectively. The axial shortening of the column has increased with time by a factor of almost four.

4.3.3 Example application (SSM) – Approach 2 In approach 2, the concrete constitutive relationship is manipulated so that the concrete stress at the end of each time instant is obtained directly. If the rectangular approximation of the integral-type creep law is used, Eq. 4.13c may be rearranged as follows: εj − εsh,j = Jj,0 σc,0 +

j

Jj,i σc,i

i=1 j−1

= Jj,0 σc,0 + Jj,j σc,j − σc,j−1 + Jj,i σc,i − σc,i−1 i=1

= Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 +

j−1 i=1

Jj,i σc,i −

j−1 i=1

Jj,i σc,i−1

Uncracked sections 115 j−1

= Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 +

i=1

j−2

Jj,i σc,i −

Jj,i+1 σc,i

i=0

j−2 = Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 + Jj,j−1 σc,j−1 + Jj,i − Jj,i+1 σc,i − Jj,1 σc,0 i=1 j−1

= Jj,0 σc,0 + Jj,j σc,j +

Jj,i − Jj,i+1 σc,i − Jj,1 σc,0 i=1 j−1

Jj,i − Jj,i+1 σc,i = Jj,j σc,j + Jj,0 − Jj,1 σc,0 + i=1

and therefore: j−1 Jj,i − Jj,i+1 σc,i εj − εsh,j = Jj,j σc,j +

(4.24)

i=0

Expressing Eq. 4.24 in terms of the stress at the end of the j-th time step, the constitutive relationship for the concrete at any time τj becomes: σc,j =

εj − εsh,j Jj,j

−

j−1 Jj,i − Jj,i+1 i=0

Jj,j

j−1

σc,i

= Ec,j εj − εsh,j + Fe,j,i σc,i

(4.25)

i=0

where Ec,j is the instantaneous elastic modulus of concrete at τj ; Fe,j,i is the stress modiﬁcation factor; and these terms are deﬁned as Ec,j =

1 Jj,j

(4.26a)

and Fe,j,i =

Jj,i+1 − Jj,i Jj,j

(4.26b)

For completeness, the corresponding expressions for Ec,j and Fe,j,i to be used in Eq. 4.25 when adopting the trapezoidal approximation of the integral-type creep law are: For i = 0: 1 Ec,j = (4.26c) Jj,j and Fe,j,i =

Jj,1 − Jj,0 Jj,j + Jj,j−1

(4.26d)

For i > 0: Ec,j =

2 Jj,j + Jj,j−1

(4.26e)

116 Uncracked sections and Fe,j,i =

Jj,i+1 − Jj,i−1 Jj,j + Jj,j−1

(4.26f)

Noting that the steel and concrete strains are always identical, the equilibrium equation at the end of the j-th time step for the axially loaded column example can be expressed as: P = σc,j Ac + σs,j As = Ac Ec,j εj − Ac Ec,j εsh,j +

j−1

Ac Fe,j,i σc,i + As Es εj

(4.27)

i=0

where σs,j = σs (τj ) and εj (= εs,j ) is the strain in both the concrete and the steel at τj . Solving for the concrete strain εj gives: j−1

εj =

Ac Ec,j εsh,j Ac Fe,j,i P + − σc,i Ac Ec,j + As Es Ac Ec,j + As Es Ac Ec,j + As Es

(4.28)

i=0

and observing that Ac Ec,j = Ac Ec,j + As Es

1 1 = Es As 1 + nj ρ 1+ Ec,j Ac

Eq. 4.28 can be rewritten as: ⎞ ⎛ j−1 Fe,j,i 1 ⎝ P εj = + εsh,j − σc,i ⎠ 1 + nj ρ Ac Ec,j Ec,j

(4.29)

i=0

It is also noted that: Jj,i+1 − Jj,i Fe,j,i 1 1 1 1 − = = Jj,j = Jj,i+1 − Jj,i = − Ec,j Jj,j Ee,j,i+1 Ee,j,i Ee τj , τi+1 Ee τ j , τ i =

ne,j,i+1 ne,j,i − Es Es

where ne,j,i = Es /Ee,j,i and, for ease of notation, Ee,j,i = Ee (τj , τi ). Eq. 4.29 can therefore be simpliﬁed to: ⎞ ⎛ j−1 ne,j,i+1 − ne,j,i 1 ⎝ P + εsh,j − σc,i ⎠ εj = 1 + nj ρ Ac Ec,j Es i=0

(4.30)

Uncracked sections 117 Substituting Eq. 4.30 into Eq. 4.25 gives: ⎞ ⎛ j−1 j−1 ne,j,i+1 −ne,j,i 1 ⎝P ⎠ +Ec,j εsh,j −Ec,j σc,i −Ec,j εsh,j + Fe,j,i σc,i σc,j = 1+nj ρ Ac Es i=0

=

i=0

j−1

ne,j,i+1 −ne,j,i 1 P −nj ρ Ec,j εsh,j −Ec,j σc,i 1+nj ρ Ac Es i=0

+

j−1

Fe,j,i σc,i +nj ρ

i=0

j−1

Fe,j,i σc,i

i=0

which can be simpliﬁed to: ⎡ ⎤ j−1 1 ⎣P − Es ρ εsh,j + ρ ne,j,i+1 − ne,j,i σc,i ⎦ σc,j = 1 + nj ρ Ac

(4.31)

i=0

With the concrete stress σc,j at time, τj , calculated from Eq. 4.31, the steel stress is obtained from the equilibrium equation: σs,j =

P − σc,j Ac As

(4.32)

and the steel and concrete strains are obtained from Eqs 4.18b and 4.17, respectively.

Example 4.3 The column analysed in Example 4.2 is to be re-analysed here using approach 2. As before, P = −1000 kN; Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; Es = 200 GPa and the time varying concrete properties are: j

0

1

2

3

4

5

6

τj (days)

14

24

44

84

214

514

10,014

t − τj (days)

0

10

30

70

200

500

10,000

ϕ(τj , τ0 ) ϕ(τj , τ1 ) ϕ(τj , τ2 ) ϕ(τj , τ3 ) ϕ(τj , τ4 ) ϕ(τj , τ5 )

0

0.53 0

0.98 0.72 0

1.38 1.18 0.90 0

1.83 1.63 1.44 1.22 0

2.10 1.89 1.69 1.51 1.26 0

2.39 2.15 1.94 1.75 1.54 1.38

Ec (τj ) (MPa) εsh (τj ) × 10−6

26,700 27,900 28,900 29,700 30,500 31,000 31,700 0

−142

−246

−325

−407

−456

−510

118 Uncracked sections

At ﬁrst loading (τ0 ): As in Example 4.2, with Ec,0 = Ee,0 = 26.7 GPa; and n0 = Es /Ec,0 = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε0 = −361×10−6 ; εs,0 = −361×10−6 ; σc,0 = −9.67 MPa and σs,0 = −72.3 MPa.

At time instant τ1 = 24 days (time step 1 from τ0 to τ1 ): For time interval, j = 1: Ec,0 = 26.7 GPa; Ec,1 = 27.9 GPa; n1 = Es /Ec,1 = 7.17; ϕ1,0 = 0.53; Ee,1,0 = Ec,0 /(1 + ϕ1,0 ) = 17.48 GPa; ne,1,0 = Es /Ee,1,0 = 11.44; ne,1,1 = Es /Ee,1,1 = 7.17 and εsh,1 = −142 × 10−6 . From Eq. 4.31, the concrete stress at the end of the ﬁrst time step (j = 1) is: 1 −1000 × 103 σc,1 = − 200,000 × 0.02 × (−142 × 10−6 ) 1 + 7.17 × 0.02 90,000 + 0.02 × (7.17 − 11.44) × (−9.67) = −8.50 MPa. −1000 × 103 + 8.50 × 90,000 = −131 MPa; 1800 −131 Eq. 4.18b and Eq. 4.17 give: εs,1 = = −653 × 10−6 and ε1 = 200,000 −653 × 10−6 . As calculated in Example 4.2, the elastic, creep and shrinkage components of the concrete strain at time τ1 are εe,1 = −319 × 10−6 , εcr,1 = −192 × 10−6 , and εsh (τ1 ) = −142 × 10−6 . and from Eq. 4.32: σs,1 =

At time instant τ2 = 44 days (time step 2 from τ1 to τ2 ): Time interval, j = 2: Ec,0 = 26.7 GPa; Ec,1 = 27.9 GPa; Ec,2 = 28.9 GPa; n2 = Es /Ec,2 = 6.92; ϕ2,0 = 0.98; Ee,2,0 = Ec,0 /(1 + ϕ2,0 ) = 13.53 GPa; ne,2,0 = Es /Ee,2,0 = 14.78; ϕ.2,1 = 0.72; Ee,2,1 = Ec,1 /(1+ϕ2,1 ) = 16.25 GPa; ne,2,1 = Es /Ee,2,1 = 12.31; and εsh,2 = −246 × 10−6 . From Eq. 4.31, the concrete stress at the end of the ﬁrst time step (j = 1) is: 1 −1000 × 103 σc,2 = − 200,000 × 0.02 × (−246 × 10−6 ) 1 + 6.92 × 0.02 90,000 +0.02 × [(12.31 − 14.78) × (−9.67) + (6.92 − 12.31) × (−8.50)] = −7.67 MPa and from Eq. 4.32: σs,1 =

−1000 × 103 + 7.67 × 90,000 = −172 MPa. 1800

Uncracked sections 119 Eqs 4.18b and 4.17 give: εs,1 =

−172 = −860 × 10−6 and ε1 = 200,000

−860 × 10−6 . As in Example 2.2, the elastic, creep and shrinkage components of concrete strain at τ2 are εe,2 = −291 × 10−6 ; εcr,2 = −323 × 10−6 , and εsh (τ2 ) = −246 × 10−6 .

At subsequent time instants: Similarly, the stress and strain components at the end of each subsequent time step are calculated and the results are tabulated below. It can be seen that the results obtained using the SSM with approaches 1 and 2 are identical. Instant Time τj Concrete Steel Total Elastic Creep Shrinkage j (days) stress stress strain strain strain strain σc (τj ) σs (τj ) ε(τj ) εe (τj ) εcr (τj ) εsh (τj ) (MPa) (MPa) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) 0 1 2 3 4 5 6

14 24 44 84 214 514 10,014

−9.67 −8.50 −7.67 −7.04 −6.39 −6.05 −5.64

−72.3 −131 −172 −204 −236 −253 −273

−361 −653 −860 −1018 −1180 −1264 −1367

−361 −319 −291 −269 −248 −237 −225

0 −192 −323 −424 −525 −571 −632

0 −142 −246 −325 −407 −456 −510

4.4 The age-adjusted effective modulus method (AEMM) 4.4.1 Formulation A simple adjustment to the effective modulus method to account for the ageing of concrete was proposed by Trost (Ref. 6). Later the method was more rigorously formulated and further developed by Dilger and Neville (Ref. 7) and Bazant (Ref. 8). The method is sometimes called the Trost–Bazant Method (Ref. 9), but Bazant’s more descriptive title, the age-adjusted effective modulus method, is preferred here. Consider the two concrete stress histories and the corresponding creep-time curves shown in Fig. 4.6. In stress history (a), σc (τ0 ) is applied at time τ0 and subsequently held constant with time. In stress history (b), the stress σc (t) is gradually applied, beginning at τ0 and reaching a magnitude equal to σc (τ0 ) at time τk . The creep strain at any time t(> τ0 ) produced by the gradually applied stress σc (t) is signiﬁcantly smaller than that resulting from the stress σc (τ0 ) abruptly applied at τ0 , as shown. This is due to ageing. The earlier a concrete specimen is loaded, the greater the ﬁnal creep strain. A reduced creep coefﬁcient can therefore be used to calculate creep strain if stress is gradually applied. Let this reduced creep coefﬁcient be χ(t, τ0 )ϕ(t, τ0 ), where the coefﬁcient χ (t, τ0 ) is called the ageing coefﬁcient (< 1.0).

120 Uncracked sections Stress (a) Constant stress

Creep strain

ecr.a(tk,t0) ecr.b(tk,t0)

sc(t0)

(b) Gradually applied stress t0

Time, t

ecr.a(tk,t0) =

tk

t0

tk

Time, t

sc(t0) s (t ) j(tk ,t0) ; ecr.b(tk,t0) = 0 0 c(tk ,t0)j(tk ,t0) Ec(t0) Ec(t0)

Figure 4.6 Creep due to constant and variable stress histories.

The creep strain at time, t, due to a stress, σc (t), that has been gradually applied over the time interval t − τ0 , may be expressed as: εcr (t) =

σc (t) χ(t, τ0 ) ϕ(t, τ0 ) Ec (τ0 )

(4.33)

The magnitude of the ageing coefﬁcient χ (t, τ0 ) generally falls within the range 0.4 to 1.0 depending on the rate of application of the gradually applied stress in the period after τ0 . Consider the gradually reducing stress history shown in Fig. 4.7. An initial compressive stress σc (τ0 ) applied at time τ0 is reduced with time due to the application of a gradually increasing tensile stress increment σc (t). The change of stress may be due to a change of the external loads, or restraint to creep and shrinkage, or variations of temperature, or combinations of these, and is usually unknown at the beginning of an analysis. Using the AEMM, the total strain at time t may be expressed as the sum of the strains produced by σc (τ0 ) (instantaneous and creep), the strains produced by the

Stress

sc(t) = sc(t0)+ Dsc(t)

sc(t0) Dsc(t)

sc(t) t0

t

Figure 4.7 A gradually reducing stress history.

Time

Uncracked sections 121 gradually applied stress increment σc (t) (instantaneous and creep), and the shrinkage strain: ε(t) = =

σc (τ0 ) σc (t) [1 + ϕ(t,τ0 )] + [1 + χ(t, τ0 ) ϕ(t, τ0 )] + εsh (t) Ec (τ0 ) Ec (τ0 ) σc (τ0 ) σc (t) + εsh (t) + Ee (t, τ0 ) Ee (t, τ0 )

(4.34)

where Ee (t, τ0 ) is the effective modulus of Eq. 4.3 and Ee (t, τ0 ) is the age-adjusted effective modulus given by: Ee (t, τ0 ) =

Ec (τ0 ) 1 + χ(t, τ0 ) ϕ(t, τ0 )

(4.35)

With the AEMM, two analyses need to be carried out: one at ﬁrst loading (time τ0 ) and one at time t after the period of sustained stress. Unlike the EMM, the ﬁnal strain depends on the stress at ﬁrst loading σc (τ0 ) and the change in stress that occurs with time σc (t). The reinforced concrete column shown in Fig. 4.1 is to be analysed using the AEMM. As for the SSM, two approaches will also be considered here: (i) Approach 1 obtains the solution for the concrete stress at time t, σc (t), by calculating the change in stress that occurs over the entire period of sustained loading, σc (t); and (ii) Approach 2 calculated the stress at time t, σc (t), directly. Both approaches lead to the same solution and differ only in the manipulation of the governing equations. 4.4.2 Example application (AEMM) – Approach 1 The instantaneous analysis at time τ0 (immediately after the application of the axial force P, and before any creep and shrinkage has occurred) is identical to that presented earlier and the instantaneous stresses and strains are: σc (τ0 ) =

P P − σc (τ0 )Ac σc (τ0 ) σs (τ0 ) ; ε(τ0 ) = ; σs (τ0 ) = and εs (τ0 ) = Ac (1 + n0 ρ) As Ec (τ0 ) Es

where n0 = Es /Ec (τ0 ) = the modular ratio at time τ0 and ρ = As /Ac = the reinforcement ratio. As described in Section 4.2.2, the equilibrium and compatibility requirements at any time t are speciﬁed by Eqs 4.4 and 4.5, respectively: P = σc (t)Ac + σs (t)As

(4.4)

εs (t) = ε(t)

(4.5)

and

122 Uncracked sections The constitutive relationship for concrete is described by Eq. 4.34 and, as before, the steel is linear-elastic: ε(t) =

σc (τ0 ) σc (t) + εsh (t) + Ee (t, τ0 ) Ee (t, τ0 )

(4.36a)

and εs (t) =

σs (t) Es

(4.36b)

where σc (t) is the unknown time-dependent change of stress caused by creep and shrinkage. If σc (τ0 ) is compressive, the stress increment σc (t) is usually tensile. Rearranging Eqs 4.36 in terms of time-varying stresses gives: σc (t) = Ee (t, τ0 )ε(t) −

Ee (t, τ0 ) Ee (t, τ0 )εsh (t) σc (τ0 ) − Ee (t, τ0 )

(4.37a)

and σs (t) = Es εs (t)

(4.37b)

At any time, t, the concrete stress is given by: σc (t) = σc (τ0 ) + σc (t)

(4.38)

and the governing equation of the problem is obtained by substituting Eqs 4.37, 4.38 and 4.5 into Eq. 4.4 and solving for the unknown total strain ε(t): ε (t) =

1 P 1 1 + σc (τ0 ) + εsh (t) − 1 + n¯ e,0 ρ Ee (t, τ0 )Ac Ee (t, τ0 ) Ee (t, τ0 )

(4.39)

where ne,0 = Es /Ee (t, τ0 ), ρ = As /Ac , and n¯ e,0 = Es / Ee (t, τ0 ) = the age-adjusted modular ratio. By substituting Eq. 4.39 into Eq. 4.36a, the concrete stress increment σc (t) can be expressed as:

1 P σc (t) = − σc (τ0 )(1 + ne,0 ρ) − εsh (t) Es ρ 1 + n¯ e,0 ρ Ac

(4.40)

With σc (t) calculated from Eq. 4.40, the resultant steel and concrete stresses at time t are given by Eqs 4.37b and 4.38. Alternatively, these could be calculated from equilibrium considerations (Eq. 4.4). 4.4.3 Determination of the ageing coefﬁcient Numerical values for χ (t, τ0 ) can be obtained from the associated creep coefﬁcient ϕ(t, τ0 ) if the stress change σc (t) is known. Like the creep coefﬁcient, the ageing

Uncracked sections 123 coefﬁcient χ (t, τ0 ) depends on the age of the concrete at ﬁrst loading τ0 , the duration of load (t − τ0 ), the size and shape of the member, and so on. For the gradually decreasing concrete stress history when a member is subjected to a constant sustained load, the ageing coefﬁcient χ (t, τ0 ) may be obtained by rearranging and expanding Eq. 4.40. With shrinkage set to zero, χ (t, τ0 ) is given by: χ (t, τ0 ) =

σc (τ0 ) 1 1 + nρ − σc (τ0 ) − σc (t) ϕ (t, τ0 ) nρ

(4.41)

If the stress history of Fig. 4.7 is the result of pure relaxation (i.e. when the member is restrained and the strain ε(t) remains constant with time at its initial value of σc (τ0 )/Ec (τ0 )), the ageing coefﬁcient χ (t, τ0 ) may be obtained by rearranging the expanded form of Eq. 4.34: χ (t, τ0 ) =

σc (τ0 ) 1 − σc (τ0 ) − σc (t) ϕ (t, τ0 )

(4.42a)

Eq. 4.42a is commonly expressed in the literature in the following form: χ (t, τ0 ) =

Ec (τ0 ) 1 − Ec (τ0 ) − R (t, τ0 ) ϕ (t, τ0 )

(4.42b)

in which R(t, τ0 ) represents the relaxation function deﬁned as the stress at time t due to a unit strain applied at time τ0 and kept constant throughout the period τ0 to t. Values for R(t, τ0 ) can be readily calculated by applying the SSM (Eq. 4.25) to the case of a constant unit strain history beginning at τ0 . Using a step-by-step numerical analysis (Section 4.3.2) to establish the gradual loss of concrete stress with time (σc (t) = σc (t) − σc (τ0 )), ageing coefﬁcients χ (t, τ0 ) may be readily determined for the creep coefﬁcients ϕ(t, τ0 ) speciﬁed by Eq. 2.3 in Section 2.1.4. For the cross-section, concrete properties and loading details of Examples 4.1 and 4.2, the ageing coefﬁcients associated with the gradual concrete stress change under a constant external load P ﬁrst applied at age τ0 are calculated using Eq. 4.41 and shown in Fig. 4.8. Also shown in Fig. 4.8 are the ageing coefﬁcients calculated using Eq. 4.42a associated with the more rapid change in concrete stress caused by pure relaxation (i.e. when the total strain ε(t) is held constant with time and the applied load P varies as a result of relaxation). Neville et al. (Ref. 9) and others have shown that ageing coefﬁcients calculated in this way, when used in conjunction with the age-adjusted effective modulus method, provided close agreement with experimental data. Fig. 4.9 shows the variation with time of the ageing coefﬁcients obtained from the creep coefﬁcients of Eq. 2.3 for a creep problem similar to that of Examples 4.1 and 4.2. For concrete loaded in the ﬁrst few weeks after casting (such as for the curves corresponding to τ0 = 7 and 14 days in Fig. 4.9), and for load durations exceeding about 100 days, the ageing coefﬁcient is between 0.55 and 0.72 for normal strength concrete with a value of 0.65 being suitable for most practical situations where ﬁnal deformations are required. Considering how uncertain are the predictions of ϕ(t, τ0 )

124 Uncracked sections

Ageing coefficient

0.9 Constant deformation (relaxation problem)

0.8 0.7

Constant load, P (creep problem)

0.6 0.5 0.4 100

10

1000

10,000

Time after loading in days (log scale)

Figure 4.8 Ageing coefﬁcient versus time for the concrete used in Example 4.2. 1

t0 = 7 days Ageing coefficient

Ageing coefficient

1 0.9 f ʹc

Eq. 4.42 0.8

25 MPa 40 MPa

0.7 25 MPa

0.6 0.5

60 MPa 40 MPa

60 MPa

25 MPa

0.8

40 MPa 25 MPa

0.7 0.6

60 MPa 40 MPa

Eq. 4.41

t0 = 14 days

0.4 10

100

1000

10,000

10

Eq. 4.42

0.8

60 MPa

0.7 Eq. 4.41 0.6 0.5

t0 = 28 days

0.4 10

100

1000

Time after loading in days (log scale)

1000

10,000

1

f ʹc 25 MPa 40 MPa 60 MPa 25 MPa 40 MPa

Ageing coefficient

1

100

Time after loading in days (log scale)

Time after loading in days (log scale)

0.9

60 MPa

0.5

Eq. 4.41

0.4

Ageing coefficient

f ʹc

Eq. 4.42

0.9

10,000

Eq. 4.42

0.9 0.8

25 MPa

40 MPa

0.7

60 MPa f ʹc

Eq. 4.41

0.6 0.5

t0 = 100 days

0.4 10

100

1000

10,000

Time after loading in days (log scale)

Figure 4.9 Ageing coefﬁcients versus time derived from ϕ(t, τ0 ) taken from Eq. 2.3 (with th = 150 mm and interior environment).

and the other concrete properties, the following values of the ﬁnal ageing coefﬁcient are recommended for use in structural design: For concrete loaded at early ages τ0 < 20 days: χ (∞, τ0 ) = χ ∗ (τ0 ) = 0.65 for creep problems (constant load)

(4.43a)

χ(∞, τ0 ) = χ ∗ (τ0 ) = 0.80 for relaxation problems (constant deformation) (4.43b)

Uncracked sections 125 For concrete loaded at later ages τ0 > 28 days: χ (∞, τ0 ) = χ ∗ (τ0 ) = 0.75 for creep problems

(4.43c)

χ(∞, τ0 ) = χ ∗ (τ0 ) = 0.85 for relaxation problems

(4.43d)

The use of Eq. 4.43 simpliﬁes the age-adjusted effective modulus method and usually leads to good approximations of both material and structural behaviour. The inadequacies of the effective modulus method are to a large extent overcome by the introduction of the ageing coefﬁcient. Bazant (Ref. 8) pointed out that the method is theoretically exact for any problem in which strain varies proportionally with the creep coefﬁcient (provided, of course, the ageing coefﬁcient has been carefully calculated from the assumed creep coefﬁcient). Extracting χ(t, τ0 ) from Fig. 4.9 is not particularly suitable for computer application nor is it generally necessary. The approximations of Eq. 4.43 are suitable for most applications.

Example 4.4 The symmetrically reinforced column analysed in Example 4.1 (see Fig. 4.1) under a constant sustained axial load P is re-analysed here using the AEMM. As before: P = −1000 kN, Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02 and Es = 200 GPa. The variation of the creep coefﬁcient and shrinkage with time were given in Example 4.1 and, for convenience, are repeated in the following table. The ageing coefﬁcients are taken from Fig. 4.9 and are also given below. All other data as given in Example 4.1. (t − τ0 ) in days

0

10

30

70

200

500

10,000 (∞)

ϕ(t, τ0 ) χ (t, τ0 ) εsh (t − τ0 ) × 10−6

0 – 0

0.53 0.60 −142

0.98 0.64 −246

1.38 0.67 −325

1.83 0.70 −407

2.10 0.70 −456

2.39 0.69 −510

At ﬁrst loading, (t − τ0 ) = 0: ϕ(t, τ0 ) = 0 and εsh (τ0 ) = 0. As in Example 4.1: with Ec (τ0 ) = Ee (τ0 ) = 26.7 GPa; and n0 = Es /Ec (τ0 ) = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε(τ0 ) = −361 × 10−6 ; εs (τ0 ) = −361 × 10−6 ; σc (τ0 ) = −9.67 MPa and σs (τ0 ) = −72.3 MPa.

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53, χ (t, τ0 ) = 0.60 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + ϕ(t, τ0 )) = 17.48 GPa; and ne,0 = Es /Ee (t, τ0 ) = 11.44; Ee (t, τ0 ) = Ec (τ0 )/(1 + χ (t, τ0 )ϕ(t, τ0 )) = 20.27 GPa; and n¯ e,0 = Es / Ee (t, τ0 ) = 9.87.

126 Uncracked sections Eq. 4.40:

1 −1000×103 σc (t) = +9.67(1+11.44×0.02) 1+9.87 ×0.02 90,000 +142×10−6 ×200,000×0.02 = +1.12 MPa;

Eq. 4.38: Eq. 4.4: Eq. 4.36b: Eq. 4.5:

σc (t) = −9.67 +1.12 = −8.55 MPa; σs (t) = ((−1000×103 +8.55×90,000)/1800 = −128.0 MPa; εs (t) = −128.0/200,000 = −640×10−6 ; and ε(t) = −640×10−6 .

The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −320 × 10−6 and εsh (t) = −142 × 10−6 ; and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −178 × 10−6 . The results of the analyses at ﬁrst loading and throughout the period of sustained loading are provided in the following table. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) 0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.48 −6.12 −5.73

Steel stress σs (t) (MPa) −72.3 −128 −169 −200 −232 −249 −269

Total Elastic Creep Shrinkage strain strain strain strain ε(t) εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −640 −843 −1002 −1158 −1247 −1346

−361 −320 −289 −266 −242 −229 −214

0 −178 −308 −411 −509 −563 −622

0 −142 −246 −325 −407 −456 −510

By comparison, the variations of stresses and strains in this example if the approximation of Eq. 4.43 is adopted throughout (i.e. if χ (t, τ0 ) is equal to 0.65 for all values of t) are provided below. For practical purposes, the two sets of results are the same. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) 0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.45 −6.08 −5.69

Steel stress σs (t) (MPa) −72.3 −128 −169 −201 −233 −252 −271

Total Elastic Creep Shrinkage strain strain strain strain ε(t) εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −639 −843 −1004 −1166 −1258 −1355

−361 −320 −289 −265 −241 −227 −213

0 −177 −307 −413 −518 −575 −632

0 −142 −246 −325 −407 −456 −510

Uncracked sections 127 4.4.4 Example application (AEMM) – Approach 2 As discussed for the SSM, approach 2 involves expressing the constitutive relationship in terms of the initial stress σc (τ0 ) and ﬁnal stress σc (t). Eq. 4.36a is re-expressed as: ε(t) = =

σc (t) − σc (τ0 ) σc (τ0 ) + + εsh (t) Ee (t, τ0 ) Ee (t, τ0 ) σc (τ0 )ϕ(t, τ0 )[1 − χ(t, τ0 )] σc (t)[1 + χ (t, τ0 )ϕ(t, τ0 )] + + εsh (t) Ec (τ0 ) Ec (τ0 )

(4.44)

and rearranging gives: Ee (t, τ0 )[ε(t) − εsh (t)] + σc (τ0 ) Fe,0 σc (t) =

(4.45)

where Fe,0 = ϕ(t, τ0 )

[χ(t, τ0 ) − 1] [1 + χ (t, τ0 )ϕ(t, τ0 )]

(4.46)

The steel stress is given by Eq. 4.37b: σs (t) = Es εs (t) and, from Eqs 4.4 and 4.5, the equilibrium and compatibility requirements at time t are: P = σc (t)Ac + σs (t)As and εs (t) = ε(t) Solving for ε(t) gives: 1 ε(t) = 1 + n¯ e,0 ρ

σc (τ0 ) Fe,0 n¯ e,0 − + εsh (t) Es Ac Ee (t, τ0 ) P

(4.47)

By substituting Eqs 4.45, 4.37b and 4.5 into Eq. 4.4, the concrete stress at time t can be expressed as: σc (t) =

1 1 + n¯ e,0 ρ

P + σc (τ0 ) Fe,0 n¯ e,0 ρ − εsh (t) Es ρ Ac

(4.48)

where ρ = As /Ac , and n¯ e,0 = Es /Ee (t, τ0 ) = the age-adjusted modular ratio. The steel stress σs (t) is determined by substituting εs (t) = ε(t) into Eq. 4.37b or by enforcing the requirements of equilibrium (Eq. 4.4).

128 Uncracked sections

Example 4.5 Example 4.4 is repeated here using the AEMM approach 2. As before: Ec (τ0 ) = Ee (τ0 ) = 26.7 GPa; σc (τ0 ) = −9.67 MPa; σs (τ0 ) = −72.3 MPa; εs (τ0 ) = −361 × 10−6 and ε(τ0 ) = −361 × 10−6 .

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53, χ (t, τ0 ) = 0.60 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + χ (t, τ0 )ϕ(t, τ0 )) = 20.27 GPa; and n¯ e,0 = Es / Ee (t, τ0 ) = 9.87. [0.60 − 1] From Eq. 4.46: Fe,0 = 0.53 = −0.160 [1 + 0.60 × 0.53)] Eq. 4.48 gives: 1 −1000 × 103 σc (t) = − 9.67 × (−0.160) × 9.87 × 0.02 1 + 9.87 × 0.02 90,000 + 142 × 10−6 × 200,000 × 0.02 = −8.55 MPa Eq. 4.4: Eq. 4.36b: Eq. 4.5:

σs (t) = (−1000 × 103 + 8.55 × 90,000)/1800 = −128.0 MPa; εs (t) = −128.0/200,000 = −640 × 10−6 ; and ε(t) = −640 × 10−6 .

The results of the analysis are identical to those obtained using approach 1.

4.5 The rate of creep method (RCM) 4.5.1 Formulation The rate of creep method was originally proposed by Glanville (Ref. 10) and further developed by Whitney (Ref. 11) in the early 1930s to describe the time-varying behaviour of concrete. Dischinger (Ref. 12) ﬁrst applied the method to the analysis of concrete structures. The RCM is based on the assumption that the rate of change of creep with time, dϕ(t, τ0 )/dt(≡ ϕ(t, ˙ τ )), is independent of the age at loading, τ . This means that creep curves for concrete loaded at different times are assumed to be parallel, as shown in Fig 4.10. This, of course, is not true. Better agreement with actual behaviour is obtained by assuming that creep curves for concrete loaded at different times are afﬁne rather than parallel, that is, they are assumed to have the same shape. However, by assuming that the rate of creep is independent of the age at loading, only a single creep curve is required to calculate creep strains due to any stress history.

Uncracked sections 129 j (t,t0)

j (t,t)

F

j (t,t0)

E

B Actual

D

A t0

j (t,ti) (assumed)

ti

j (t,ti) = j (t,t0)

C t

Time

Figure 4.10 Parallel creep curves assumed in the rate of creep method.

Consider the parallel creep curves of Fig. 4.10. Since the ordinates EF and CD are assumed to be equal, CD = CF – AB or: ϕ(t, τi ) = ϕ (t, τ0 ) − ϕ (τi , τ0 )

(4.49)

The creep–time curve caused by a stress applied at any age τi is thus completely deﬁned by a single curve ϕ(t, τ0 ), where τ0 is usually taken to be the age at ﬁrst loading. The creep strain at time t caused by a constant stress σc (τi ) applied at τi is therefore taken to be: εcr (t, τi ) =

σc (τi ) σc (τi ) ϕ(t, τi ) = [ϕ (t, τ0 ) − ϕ (τi , τ0 )] Ec (τ0 ) Ec (τ0 )

(4.50)

and the change in creep strain between any two time instants t1 and t2 after the loading at τi is: εcr (t, τi ) = εcr (t2 , τi ) − εcr (t1 , τi ) =

σc (τi ) [ϕ (t2 , τ0 ) − ϕ (t1 , τ0 ) ] Ec (τ0 )

(4.51)

If a continuously varying stress history is divided into small time intervals δt and the stress during each interval is considered to be constant, the change of creep strain during any time interval is given by Eq. 4.51. In the limit, as δt approaches zero, the rate of change of creep depends only on the current stress and the rate of change of the creep coefﬁcient and is given by: d εcr (t, τ ) σc (t) d ϕ (t, τ0 ) σc (t) = or ε˙ cr (t, τ ) = ϕ(t, ˙ τ0 ) dt Ec (τ0 ) dt Ec (τ0 )

(4.52)

The rate of change of the instantaneous strain at any time depends on the rate of change of stress: d εe (t) σ˙ c (t) 1 d σc (t) = or ε˙ e (t) = dt Ec (τ0 ) d t Ec (τ0 ) where the elastic modulus of concrete is here assumed to be constant in time.

(4.53)

130 Uncracked sections If it is further assumed that shrinkage develops at the same rate as creep (i.e. the creep and shrinkage curves are afﬁne), then: εsh (t) =

εsh (∞) ϕ (t, τ0 ) ϕ(∞, τ0 )

(4.54)

and the time rate of change of shrinkage is given by: ε˙ sh (t) =

ε∗ εsh (∞) ϕ˙ (t, τ0 ) = ∗ sh ϕ˙ (t, τ0 ) ϕ(∞, τ0 ) φ (τ0 )

(4.55)

The rate of change of the total concrete strain may be expressed as the sum of the rates of change of each of the three strain components given by Eqs 4.52, 4.53 and 4.55:

ε∗ σ˙ c (t) σc (t) ε˙ (t, τ ) = + ϕ(t, ˙ τ0 ) + ∗ sh (4.56) Ec (τ0 ) Ec (τ0 ) ϕ (τ0 ) This ﬁrst order differential equation is a constitutive relationship for concrete that can be readily included in structural analysis. The solution of the resulting differential equations is easily obtained for a variety of practical problems. Eq. 4.56 may be rewritten with the creep coefﬁcient ϕ (≡ ϕ (t, τ )) as the independent variable: ε∗ d ε (t, τ ) 1 d σc (t) σc (t) = + + ∗ sh dϕ Ec (τ0 ) d ϕ Ec (τ0 ) ϕ (τ0 )

(4.57)

Eqs 4.56 and 4.57 were developed by Dischinger (Ref. 12) and this type of differential constitutive relationship for concrete is often referred to as Dischinger’s equation of state. 4.5.2 Discussion The rate of creep method, although mathematically attractive, has several deﬁciencies. The assumption of parallel creep curves causes a signiﬁcant underestimation of creep in old concrete. As time increases, ϕ˙ (t, τ0 ) approaches zero and, according to the RCM, so too does the creep strain for concrete loaded at times much later than τ0 . This is not so. Old concrete does creep, albeit much less than young concrete. The RCM therefore underestimates creep for an increasing stress history. This error may be large if signiﬁcant increases of stress occur at times τi >> τ0 . Eq. 4.52 also implies that when stress is removed, the rate of change of creep is zero, that is, creep recovery is not predicted. Creep strains are therefore overestimated for a decreasing stress history. However, for the many practical situations in which loads are applied on relatively young concrete and the stress does not vary too much with time, the RCM gives excellent results. 4.5.3 Example application (RCM) The rate of creep analysis of the column shown in Fig. 4.1 follows the same general steps as the elastic analysis described in Section 4.2.2. However, since the constitutive

Uncracked sections 131 relationship for concrete is in differential form (Eq. 4.56), it is convenient to also express the equilibrium and compatibility equations in this form. For clarity, the arguments t and τ0 are omitted from the various functions in the following analysis. Noting that the rate of change of the applied load P with time is zero, differentiating the equilibrium equation with respect to time gives: ˙ c +N ˙ s = σ˙ c Ac + σ˙ s As = 0 P˙ = N

(4.58)

For compatibility, the rates of change of concrete and steel strains are identical, that is: ε˙ = ε˙ s

(4.59)

and the constitutive relationships for both the concrete and the steel are: ε˙ =

σ˙ c + ϕ˙ Ec

∗ σc εsh + ∗ Ec ϕ

and ε˙ s =

σ˙ s Es

(4.60)

∗ = ε (∞); and ϕ ∗ = ϕ (∞, τ ). From Eq. 4.58: where ϕ˙ = ϕ˙ (t, τ0 ) ; εsh 0 sh

σ˙ s = − σ˙ c

Ac σ˙ c =− As ρ

(4.61)

and substituting Eqs 4.60 and 4.61 into Eq. 4.59 gives: −

∗ σ˙ c σc εsh σ˙ c + ϕ˙ + ∗ = Es ρ E c Ec ϕ

Multiplying by Ec and gathering like terms yields: σ˙ c −nρ = ϕ˙ σc + S 1 + nρ

(4.62)

where: S=

∗ E εsh c

(4.63)

ϕ∗

Integrating both sides of Eq. 4.62 with respect to time gives: nρ ln(σc + S) tt=τ0 = − ϕ tt=τ0 1 + nρ Solving for concrete stress gives: −nρ σc (t) + S = e 1+nρ σc (τ0 ) + S

ϕ (t,τ0 )

i.e. ln

σc (t) + S nρ =− ϕ (t, τ0 ). σc (τ0 ) + S 1 + nρ

132 Uncracked sections and therefore: −nρ

σc (t) = (σc (τ0 ) + S) e 1+nρ

ϕ(t,τ0 )

−S

(4.64)

With the concrete stress obtained from Eq. 4.64, the steel stress may be found from Eq. 4.4 and the steel strain from Eq. 4.6b. Compatibility requires that the concrete strain is the same as the steel strain.

Example 4.6 The symmetrically reinforced column subjected to a constant sustained axial load P that was analysed in Example 4.1 (see Fig. 4.1) is to be re-analysed using the RCM. As before: P = −1000 kN, Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; Ec (τ0 ) = 26.7 GPa; Es = 200 GPa; n = Es /Ec (τ0 ) = 7.48; and ∗ = −510 × 10−6 . εsh The variations of the creep coefﬁcient with time is: (t − τ0 ) in days

0

10

30

70

200

500

10,000 (∞)

ϕ(t, τ0 )

0

0.53

0.98

1.38

1.83

2.10

2.39

The constants in Eq. 4.64 are: and from Eq. 4.62: S =

nρ 7.48 × 0.02 = = 0.130; 1 + nρ 1 + 7.48 × 0.02

−510 × 10−6 × 26,700 = −5.71 MPa. 2.39

At ﬁrst loading, (t − τ0 ) = 0: ϕ(t, τ0 ) = 0; εsh (t) = 0 σc (τ0 ) = −9.67 MPa; σs (τ0 ) = −72.3 MPa; εs (τ0 ) = −361 × 10−6 and ε(τ0 ) = −361 × 10−6 .

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53 Eq. 4.64: Eq. 4.4: Eq. 4.6b: Eq. 4.5:

σc (t) = (−9.67 − 5.71)e−0.130×0.53 + 5.71 = −8.65 MPa; −1000 × 10−3 + 8.65 × 90,000 = 123.3 MPa; 1800 −123.3 εs (t) = = −616 × 10−6 ; 200,000

σs (t) =

ε(t) = −616 × 10−6 .

Uncracked sections 133 The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −323 × 10−6 ; from Eq. 4.54, the shrinkage component of strain is εsh (t) = (0.53/2.39) × (−510 × 10−6 ) = −113 × 10−6 (since the creep and shrinkage curves are assumed to be afﬁne); and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −180 × 10−6 . It is noted that in this example using RCM, because of the assumption that the creep and shrinkage curves have the same shape, different levels of shrinkage from those speciﬁed in the previous examples occur during each time step. The results of the analyses at ﬁrst loading and throughout the period of sustained loading are as follows: Time t (days)

Duration of load t − τ0 (days)

Concrete stress σc (t) (MPa)

Steel stress σs (t) (MPa)

14 24 44 84 214 514 10,014

0 10 30 70 200 500 10,000

−9.67 −8.65 −7.83 −7.14 −6.41 −5.99 −5.56

−72.3 −123 −164 −198 −235 −256 −278

Total Elastic strain concrete ε(t) strain εe (t) (×10−6 ) (×10−6 ) −361 −616 −820 −992 −1175 −1279 −1388

−361 −323 −293 −267 −240 −224 −208

Creep Shrinkage strain strain εcr (t) εsh (t) (×10−6 ) (×10−6 ) 0 −180 −319 −431 −544 −607 −670

0 −113 −209 −294 −391 −448 −510

4.6 Comparison of methods of analysis A comparison of the numerical results calculated using each method of analysis for the axially loaded column section considered in Examples 4.1–4.6 is provided in Table 4.1. The prediction of time-dependent redistribution of stresses and the gradual development of creep strain with time are compared in Figs 4.11 and 4.12, respectively. A large redistribution of stresses is predicted by all of the methods of analysis. In this axially loaded column, the concrete stress decreases substantially with time and the steel stress increases dramatically. At initial loading, the concrete in the section carried 87 per cent of the total load. After 10,000 days under load, this has reduced to 59.3 per cent (according to the AEMM, for example). During this same time period, the steel stress increased from 72.3 MPa to 269 MPa. This is, in fact, typical of the redistribution of stresses that takes place with time in reinforced concrete structures. The concrete and steel stresses obtained using the AEMM at any time t are almost identical with those predicted by the much more laborious SSM (calculated with 18 intervals). This is not surprising; since the ageing coefﬁcients were determined from the concrete stress changes calculated using the SSM. However, if one assumes that the ageing coefﬁcient is constant and equal to 0.65 at every value of t, as suggested by Eq. 4.43, the AEMM predicts stresses and total strains to within 1 per cent of these more reﬁned values.

134 Uncracked sections Table 4.1 Comparisons of calculated stresses and strains (Examples 4.1–4.6) Method of analysis

Duration of load (days)

Concrete stress σc (τi ) (MPa)

Steel stress σs (τi ) (MPa)

Total strain ε(τi ) (×10−6 )

Elastic strain εe (τi ) (×10−6 )

Creep strain εcr (τi ) (×10−6 )

Shrinkage strain εsh (τi ) (×10−6 )

Effective modulus method (EMM)

0 10 30 70 200 500 10,000

−9.67 −8.58 −7.82 −7.23 −6.66 −6.35 −6.02

−72.3 −127 −165 −194 −222 −238 −255

−361 −633 −824 −969 −1112 −1191 −1273

−361 −321 −292 −270 −249 −237 −225

0 −170 −285 −374 −456 −497 −538

0 −142 −246 −325 −407 −456 −510

Ageadjusted effective modulus method (AEMM)

0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.48 −6.12 −5.73

−72.3 −128 −169 −200 −232 −249 −269

−361 −640 −843 −1002 −1158 −1247 −1346

−361 −320 −289 −266 −242 −229 −214

0 −178 −308 −411 −509 −563 −622

0 −142 −246 −325 −407 −456 −510

0 10 30 70 200 500 10,000

−9.67 −8.55 −7.72 −7.09 −6.46 −6.10 −5.71

−72.3 −128 −169 −201 −233 −251 −270

−361 −641 −847 −1006 −1164 −1253 −1349

−361 −320 −292 −270 −249 −238 −226

0 −179 −309 −411 −508 −559 −613

0 −142 −246 −325 −407 −456 −510

0 10 30 70 200 500 10,000

−9.67 −8.65 −7.83 −7.14 −6.41 −5.99 −5.56

−72.3 −123 −164 −198 −235 −256 −278

−361 −616 −820 −992 −1175 −1279 −1388

−361 −323 −293 −267 −240 −224 −208

0 −180 −319 −431 −544 −607 −670

0 −113 −209 −294 −391 −448 −510

Step-by-step method (SSM)

Rate of creep method (RCM)

Figure 4.12 conﬁrms that the EMM underestimates creep strains for a decreasing stress history, predicting full creep recovery as the stress reduces. The EMM predicts the smallest creep strain at any time t > τ and the smallest eventual stress redistribution (see Fig. 4.11). By contrast, the RCM overestimates creep for this decreasing stress history because it does not allow for any creep recovery. The RCM predicts the largest creep strain and the largest stress redistribution. However, for this simple example, good results are obtained using the RCM at all times after loading with relatively little computational effort. It is noted that the magnitudes of the stresses and deformations predicted by the SSM and the AEMM lie between the magnitudes predicted by the EMM (which is known to underestimate the effects of creep for a decreasing stress history) and the magnitudes predicted by the RCM (which is known to overestimate the effects of creep). Although the total strain predicted by the AEMM and the SSM are almost identical, the elastic strain is different. The AEMM assumes that the total change of stress is applied at τ0 and so the elastic strain at any time t is taken as the concrete stress at that time divided

Uncracked sections 135

Concrete stress (MPa)

−10 EMM AEMM SSM RCM

−8

−6

−4 200

0

400 600 Duration of load (t − t) (days)

1000

Steel stress (MPa)

−300

−200 EMM AEMM SSM RCM

−100

0 0

200

400 600 Duration of load (t − t) (days)

1000

Figure 4.11 Stress redistributions in axially loaded column examples.

Creep strain (×10−6)

−750

−500 EMM AEMM SSM RCM

−250

0 0

200

400

600

1000

Duration of load (t − t) (days)

Figure 4.12 Creep strain versus time in the axially loaded column examples.

136 Uncracked sections by the elastic modulus at τ0 . In the SSM, the elastic strain caused by a change of stress at any time t(> τ0 ) is calculated using the elastic modulus at that time. Therefore, in the example considered here, with a decreasing stress history, the AEMM slightly underestimates the elastic strain predicted by the SSM and, as a consequence, slightly overestimates the creep strain. The results from the SSM depend on the number of time steps considered and the shape of the numerous creep coefﬁcient versus time curves required for the analysis. More accurate results are obtained as the number of time steps increases. The increased amount of input data required and the considerable extra computational effort associated with the SSM normally make it suitable only for computer applications. For manual calculations, the AEMM has much to recommend it. It is usually the most satisfactory alternative in terms of both efﬁciency and accuracy and can be easily incorporated into most existing structural analysis packages.

4.7 References 1. Faber, O. (1927). Plastic yield, shrinkage and other problems of concrete and their effects on design. Minutes of the Proceedings of the Institution of Civil Engineers, 225, Part I, London, 27–23. 2. Ghali, A., Neville, A.M. and Jha, P.C. (1967). Effect of elastic and creep recoveries of concrete on loss of prestress. ACI Journal, 64, 802–810. 3. Comité Euro-International du Béton (1984). CEB Design Manual on Structural Effects of Time-Dependent Behaviour of Concrete. Georgi Publishing, Saint-Saphorin, Switzerland. 4. Ghali, A., Favre, R. and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London. 5. Kawano, A. and Warner, R.F. (1996). Model formulations for numerical creep calculations for concrete. Journal of Structural Engineering, 122(3), 284–290. 6. Trost, H. (1967). Auswirkungen des Superpositionsprinzips auf Kriech- und RelaxationsProbleme bei Beton und Spannbeton. Beton- und Stahlbetonbau, 62(10), 230–238, No. 11, 261–269. 7. Dilger, W. and Neville, A.M. (1971). Method of creep analysis of structural members. ACI SP 27-17, 349–379. 8. Bazant, Z.P. (1972). Prediction of concrete creep effects using age-adjusted effective modulus method. ACI Journal, 69, April, 212–217. 9. Neville, A.M., Dilger, W.H. and Brooks, J.J. (1983). Creep of Plain and Structural Concrete. Construction Press (Longman Group Ltd), London. 10. Glanville, W.H. (1930). Studies in Reinforced Concrete – III, The Creep or Flow of Concrete under Load. Building Research Technical Paper No. 12, Department of Scientiﬁc and Industrial Research, London. 11. Whitney, C.S. (1932). Plain and reinforced concrete arches. ACI Journal, 28, 479–519. 12. Dischinger, F. (1937). Untersuchungen über die Knicksicherheit, die elastische Verformung und das Kriechen des Betons bei Bogenbrücken. Der Bauingenieur, 18(33/34), 487–529 and No. 35/36, 539–552 and No.39/40, 595–621.

5

Uncracked sections Axial force and uniaxial bending

5.1 Introductory remarks In this chapter, time analyses are presented for a variety of uncracked cross-sections containing at least one axis of symmetry and subjected to axial load and uniaxial bending. The concrete is assumed to be able to carry any applied tension and is therefore uncracked. Symmetrically reinforced and asymmetrically reinforced sections containing any number of levels of both non-prestressed and prestressed reinforcement are considered. Composite steel–concrete and composite concrete–concrete sections are also examined. The proposed methods of analysis are based on the assumptions of the Euler– Bernoulli beam theory, in which plane sections are assumed to remain plane and perpendicular to the beam axis before, and after, both short- and long-term deformations. This means that the strain distributions on the cross-section, both immediately upon loading and after a prolonged period of sustained loading and shrinkage, are assumed to be linear.

5.2 Overview of cross-sectional analysis Cross-sectional analysis is used extensively for modelling structural response at both service and ultimate load conditions. With this approach, the governing equilibrium equations describing the behaviour of any cross-section are expressed in terms of two unknowns that deﬁne the strain diagram. These unknowns can be identiﬁed by a single value of strain measured at the level of the reference axis εr and the slope of the strain diagram κ (which is, of course, the curvature of the cross-section). Considering the cross-section shown in Fig. 5.1a, the section is symmetrical about the y-axis and the orthogonal x-axis is selected as the reference axis. If the cross-section is subjected to an axial force applied at the origin of the x- and y-axes and a bending moment applied about the x-axis, the strain diagram is shown in Fig. 5.1b and the strain at any depth y below the reference axis is given by: ε = εr + yκ

(5.1)

The two unknowns of the problem, εr and κ, are then determined by enforcing horizontal and rotational equilibrium at the cross-section: Ni = Ne

(5.2a)

138 Uncracked sections er e

x Area, A y (a) Cross-section

k

y (b) Strain diagram

Figure 5.1 Generic cross-section.

and Mi = Me

(5.2b)

where Ne and Me denote the external axial force and moment, respectively, at the section and Ni and Mi are the internal axial force and moment, respectively, given by: Ni =

A

σ dA

(5.3a)

yσ dA

(5.3b)

and Mi =

A

When the two unknowns (εr and κ) are calculated from the two equilibrium equations (Eqs 5.2) and the strain is determined using Eq. 5.1, the stresses in the concrete and steel may be obtained from the appropriate constitutive relationships. The internal actions are then readily determined from the stresses using Eqs 5.3. This procedure forms the basis of both the short- and long-term analyses presented in the remainder of this chapter.

5.3 Short-term analysis of reinforced or prestressed concrete cross-sections The short-term analysis of an uncracked reinforced or prestressed concrete crosssection at service loads is usually made assuming linear-elastic behaviour of the concrete (in compression and tension) and linear-elastic behaviour of the nonprestressed reinforcement and the prestressing steel. The procedure can be applied to typical cross-sections such as those shown in Fig. 5.2. Without any loss of generality, it is assumed that the contribution of each reinforcing bar or prestressing tendon is lumped into layers according to its location, as shown in Fig. 5.3. The numbers of layers of non-prestressed and prestressed reinforcement are ms and mp , respectively. In Fig. 5.3b, ms = 3 and mp = 2. In particular, the properties of each layer of non-prestressed reinforcement are deﬁned by its area, elastic modulus and location with respect to the arbitrarily chosen x-axis and are labelled as As(i) , Es(i) and

Uncracked sections 139

Typical prestressed steel reinforcement

Typical non-prestressed steel reinforcement

Figure 5.2 Typical reinforced and prestressed concrete sections.

ys(i) , respectively. With this notation the subscript ‘s’ stands for (non-prestressed) steel reinforcement and i = 1, . . . , ms . Similarly, Ap(i) , Ep(i) and yp(i) represent, respectively, the area, elastic modulus and location of the prestressing steel with respect to the x-axis and i = 1, . . . , mp . The geometric properties of the concrete part of the cross-section are Ac , Bc and Ic , which denote the area and the ﬁrst and second moments of area of the concrete about the x-axis, respectively. For the short-term or instantaneous analysis, assumed to take place at time τ0 , the linear-elastic stress-strain relationships of the concrete and the steel are: σc,0 = Ec,0 ε0

(5.4a)

σs(i),0 = Es(i) ε0 σp(i),0 = Ep(i) ε0 + εp(i),init

(5.4b) (5.4c)

in which σc,0 , σs(i),0 and σp(i),0 represent the stresses in the concrete, in the i-th layer of non-prestressed reinforcement (with i = 1, . . . , ms ) and in the i-th layer of prestressing steel (with i = 1, . . . , mp ), respectively, immediately after ﬁrst loading at time τ0 , while

Non-prestressed steel reinforcement ds(1) ys(1) ys(2)

ds(2) Concrete

As(1) As(2)

Ac, Bc, Ic dp(1) dp(2) ds(3)

x

Prestressed steel reinforcement Non-prestressed steel reinforcement

yp(1) yp(2)

Ap(1) Ap(2) As(3)

ys(3)

y (a) Generic cross-section

(b) The contribution of each reinforcement bar or tendon is lumped into layers located ys(i) and yp(i) from the reference axis (x-axis)

Figure 5.3 Generic cross-section and arrangement of reinforcement.

140 Uncracked sections εp(i),init is the initial strain in the i-th layer of prestressing steel produced by the initial tensile prestressing force Pp(i),init (i.e. the prestressing force before the prestress is transferred to the concrete) and given by: εp(i),init =

Pp(i),init Ap(i) Ep(i)

(5.5)

With this method, the prestressing force is included in the analysis by means of an induced strain εp(i),init rather than as an external action (Refs 1 and 2). For the short-term analysis at time τ0 , the internal axial force and moment resisted by the cross-section about the reference axis are denoted Ni,0 and Mi,0 , respectively. The internal axial force Ni,0 is the sum of the axial forces resisted by the component materials forming the cross-section and is given by: Ni,0 = Nc,0 + Ns,0 + Np,0

(5.6)

where Nc,0 , Ns,0 and Np,0 represent the axial forces resisted by the concrete, the nonprestressed reinforcement and the prestressing steel, respectively, and are calculated from: Nc,0 = Ns,0 =

Ac

σc,0 dA =

Ac

Ec,0 (εr,0 + yκ0 ) dA = Ac Ec,0 εr,0 + Bc Ec,0 κ0

(5.7a)

ms ms ms As(i) Es(i) εr,0 + ys(i) κ0 = As(i) Es(i) εr,0 + ys(i) As(i) Es(i) κ0 i=1

i=1

i=1

(5.7b) mp mp mp Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(i) Ep(i) εp(i),init Np,0 = i=1

i=1

(5.7c)

i=1

where the additional subscripts ‘0’ used for the strain at the level of the reference axis (εr,0 ) and the curvature (κ0 ) highlight that these are calculated at time τ0 after the application of Ne,0 and Me,0 and after the transfer of prestress. By substituting Eqs 5.7 into Eq. 5.6, the equation for Ni,0 is expressed in terms of the actual geometry and elastic moduli of the materials forming the cross-section: Ni,0 = Ac Ec,0 +

ms

As(i) Es(i) +

i=1

+ Bc Ec,0 +

ms

mp

Ap(i) Ep(i) εr,0

i=1

ys(i) As(i) Es(i) +

mp

yp(i) Ap(i) Ep(i) κ0 +

i=1

i=1

mp Ap(i) Ep(i) εp(i),init i=1

mp

= RA,0 εr,0 + RB,0 κ0 +

Ap(i) Ep(i) εp(i),init i=1

(5.8)

Uncracked sections 141 in which RA,0 and RB,0 represent, respectively, the axial rigidity and the stiffness related to the ﬁrst moment of area about the reference axis calculated at time τ0 and are given by: RA,0 = Ac Ec,0 +

ms

As(i) Es(i) +

mp

i=1

RB,0 = Bc Ec,0 +

ms

Ap(i) Ep(i)

(5.9a)

i=1

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

(5.9b)

i=1

Similarly, the equation for Mi,0 may be expressed as: mp ms Mi,0 = Bc Ec,0 + ys(i) As(i) Es(i) + yp(i) Ap(i) Ep(i) εr,0

i=1

+ Ic Ec,0 +

ms

i=1 mp 2 ys(i) As(i) Es(i) +

i=1

+

2 yp(i) Ap(i) Ep(i)

κ0

i=1

mp yp(i) Ap(i) Ep(i) εp(i),init i=1

= RB,0 εr,0 + RI,0

mp yp(i) Ap(i) Ep(i) εp(i),init κ0 +

(5.10)

i=1

where RI,0 is the ﬂexural rigidity at time τ0 given by: RI,0 = Ic Ec,0 +

ms i=1

2 ys(i) As(i) Es(i) +

mp

2 yp(i) Ap(i) Ep(i)

(5.11)

i=1

Substituting the expressions for Ni,0 and Mi,0 (Eqs 5.8 and 5.10) into Eqs 5.2 produces the system of equilibrium equations that may be written in compact form as: re,0 = D0 ε0 + fp,init

(5.12)

where

Ne,0 re,0 = Me,0

RA,0 RB,0 D0 = RB,0 RI,0

εr,0 ε0 = κ0 mp Ap(i) Ep(i) εp(i),init fp,init = yp(i) Ap(i) Ep(i) εp(i),init i=1

(5.13a) (5.13b) (5.13c)

(5.13d)

142 Uncracked sections The vector re,0 is the vector of the external actions at ﬁrst loading (at time τ0 ), i.e. axial force Ne,0 and moment Me,0 ; the matrix D0 contains the cross-sectional material and geometric properties calculated at τ0 ; the strain vector ε0 contains the unknown independent variables describing the strain diagram at time τ0 (εr,0 and κ0 ); and the vector f p,init contains the actions caused by the initial prestressing. The vector ε0 is readily obtained by solving the equilibrium equations (Eq. 5.12) giving: re,0 − fp,init = F0 re,0 − fp,init (5.14) ε0 = D−1 0 where F0 =

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

−RB,0 RA,0

(5.15)

The stress distribution related to the concrete and reinforcement can then be calculated from the constitutive equations (Eqs 5.4) re-expressed here as: σc,0 = Ec,0 ε0 = Ec,0 [1

y]ε0

σs(i),0 = Es(i) ε0 = Es(i) [1 ys(i) ]ε0 σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) [1

(5.16a) (5.16b) yp(i) ] ε0 + Ep(i) εp(i),init

(5.16c)

where ε0 = εr,0 + yκ0 = [1 y] ε0 . Although this procedure is presented here assuming linear-elastic material properties, it is quite general and is also applicable to non-linear material behaviour, in which case the integrals of Eqs 5.3 might have to be evaluated numerically. However, when calculating the short-term response of uncracked reinforced and prestressed concrete cross-sections under typical in-service loads, material behaviour is essentially linear elastic. In reinforced and prestressed concrete design, it is common to calculate the crosssectional properties by transforming the section into equivalent areas of one of the constituent materials. For example, for the cross-section of Fig. 5.3a, the transformed concrete cross-section for the short-term analysis is shown in Fig. 5.4, with the area of each layer of bonded steel reinforcement and tendons (As(i) and Ap(i) , respectively) transformed into equivalent areas of concrete (ns(i),0 As(i) and np(i),0 Ap(i) , respectively), where ns(i),0 = Es(i) /Ec,0 is the modular ratio of the i-th layer of non-prestressed steel and np(i),0 = Ep(i) /Ec,0 is the modular ratio of the i-th layer of prestressing steel. For the transformed section of Fig. 5.4, the cross-sectional rigidities deﬁned in Eqs 5.9 and 5.11 can be re-calculated as: RA,0 = A0 Ec,0

(5.17a)

RB,0 = B0 Ec,0

(5.17b)

RI,0 = I0 Ec,0

(5.17c)

where A0 is the area of the transformed concrete section, and B0 and I0 are the ﬁrst and second moments of the transformed area about the reference x-axis at ﬁrst loading.

Uncracked sections 143 (ns(1),0 −1)As(1) (ns(2),0 −1)As(2)

x (np(1),0 −1)A(1) (np(2),0 −1)Ap(2)

if bonded

(ns(3),0 −1)As(3)

y

Figure 5.4 Transformed section with bonded reinforcement transformed into equivalent areas of concrete.

Substituting Eqs 5.17 into Eq. 5.15 enables F0 to be expressed in terms of the properties of the transformed concrete section as:

I0 F0 = 2 Ec,0 (A0 I0 − B0 ) −B0 1

−B0 A0

(5.18)

The two approaches proposed for the calculation of the cross-sectional rigidities, i.e. the one based on Eqs 5.9 and 5.11 and the one relying on the properties of the transformed section (Eqs 5.17), are equivalent. The procedure based on the transformed section (Eqs 5.17) is often preferred for the analysis of reinforced and prestressed concrete sections, while for composite steel–concrete and concrete–concrete cross-sections, the procedure based on Eqs 5.9 and 5.11 is generally more convenient. The use of both approaches is illustrated in the following examples.

Example 5.1 For the reinforced concrete section shown in Fig. 5.5, the strain and stress distributions are to be determined immediately after application of an axial force Ne,0 = −30 kN and a sagging (positive) bending moment of Me,0 = 50 kNm, applied with respect to the x-axis located 200 mm below the top ﬁbre of the cross-section. Both the concrete and reinforcement are assumed to be linearelastic with Ec,0 = 25 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = ns(1),0 = ns(2),0 = Es /Ec,0 = 8. For this reinforced concrete cross-section, f p,init is a nil vector and the vector of external actions is: −30 × 103 N re,0 = 50 × 106 Nmm

144 Uncracked sections b = 300 ds(1) = 50 As(1) = 620 mm2 dref = 200 x D = 600

ys(1) = −150 ys(2) = +350

ds(2) = 550

As(2) = 1800 mm2

y

Figure 5.5 Reinforced concrete cross-section for Example 5.1 (dimensions in mm).

With the steel reinforcement transformed into equivalent areas of concrete, the relevant properties of the transformed cross-section for inclusion in the F0 matrix (Eq. 5.18) are calculated as follows: A0 = bD + (ns,0 − 1)[As(1) + As(2) ] = 300 × 600 + (8 − 1) × [620 + 1800] = 196,900 mm2

D B0 = bD − dref + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] 2 = 300 × 600 × (300 − 200) + (8 − 1) × [620 × (−150) + 1800 × 350] = 21,760 × 103 mm3

2 bD3 D 2 2 I0 = + bD − dref + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] 12 2 =

300 × 6003 + 300 × 600 (300 − 200)2 + (8 − 1) 12 × [620 × (−150)2 + 1800 × 3502 ] = 8841 × 106 mm4

From Eq. 5.18: F0 =

1 25,000 × (196,900 × 8841 × 106 − (21,760 × 103 )2 ) −21,760 × 103 8841 × 106 × 196,900 −21,760 × 103

278.9 × 10−12 N−1 −686.5 × 10−15 N−1 mm−1 = −1 −686.5 × 10−15 N mm−1 6.214 × 10−15 N−1 mm−2

Uncracked sections 145 The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.14:

! −30 × 103 0 278.9 × 10−12 −686.5 × 10−15 ε0 = × − 0 −686.5 × 10−15 6.214 × 10−15 50 × 106

−42.7 × 10−6 = 0.331 × 10−6 mm−1

The strain at the reference axis and the curvature are therefore: εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 and, from Eq. 5.1, the top (y = −200 mm) and bottom (y = +400 mm) ﬁbre strains are: ε0(top) = εr,0 − 200 × κ0 = (−42.7 − 200 × 0.331) × 10−6 = −108.9 × 10−6 ; and ε0(btm) = εr,0 + 400 × κ0 = (−42.7 + 400 × 0.331) × 10−6 = +89.8 × 10−6 . The top and bottom ﬁbre stresses in the concrete and the stresses in the two layers of reinforcement are obtained from Eqs 5.16:

σc,0(top) = Ec,0 1 yc(top)

= −2.72 MPa

σc,0(btm) = Ec,0 1 yc(btm) = 2.25 MPa

σs(1),0 = Es(1) 1 ys(1)

σs(2),0 = Es(2) 1 ys(2) = 14.6 MPa

−42.7 × 10−6 ε0 = 25 × 10 × 1 400 0.331 × 10−6

3

−42.7 × 10−6 ε0 = 200 × 10 × 1 −150 0.331 × 10−6

−42.7 × 10−6 ε0 = 200 × 10 1 350 0.331 × 10−6

= −18.5 MPa

−42.7 × 10−6 ε0 = 25 × 10 × 1 −200 0.331 × 10−6

3

3

3

146 Uncracked sections The results are plotted in Fig. 5.6.

er,0 = −42.7 × 10−6

− 2.72 −18.5 e

x

s

k0 = 0.331 × 10−6 mm−1

14.6 y

y

(a) Cross-section

y

(b) Strain diagram

2.25

(c) Stress diagram (MPa)

Figure 5.6 Strain and stress diagrams for Example 5.1.

The cross-sectional rigidities could have also been calculated using Eqs 5.9 and 5.11 without transforming the section as follows:

RA,0 = Agross Ec,0 +

ms

As(i) (Es(i) −Ec,0 ) = bDEc,0 + As(1) + As(2) (Es − Ec,0 )

i=1

= 300 × 600 × 25,000 + (620 + 1800) × (200,000 − 25,000) = 4923 × 106 N RB,0 = Agross

ms D − dref Ec,0 + ys(i) As(i) (Es(i) − Ec,0 ) 2 i=1

= 300 × 600 ×

600 − 200 × 25,000 + [620 × (−150) + 1800 × 350] 2

× (200,000 − 25,000) = 543.9 × 109 Nmm RI,0 = Igross + Agross

D − dref 2

2 Ec,0 +

ms

2 ys(i) As(i) (Es(i) − Ec,0 )

i=1

300 × 6003 2 = + 300 × 600 (300 − 200) × 25,000 + 620 × (−150)2 12 +1800 × 3502 × (200,000 − 25,000) = 221.0 × 1012 Nmm2

Uncracked sections 147 and F0 can then be obtained from Eq. 5.15 as: F0 = =

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

−RB,0 RA,0

1

2 543.9 × 109 −543.9 × 109 4923 × 106

4923 × 106 × 221.0 × 1012 −

×

221.0 × 1012 −543.9 × 109

278.9 × 10−12 N−1 = −686.5 × 10−15 N−1 mm−1

−686.5 × 10−15 N−1 mm−1 6.214 × 10−15 N−1 mm−2

and this, of course, is identical to that calculated previously using Eq. 5.18.

Example 5.2 The instantaneous stress and strain distributions on the precast pretensioned concrete section shown in Fig. 5.7 are to be calculated. The cross-section is that of a Girder Type 3 from the AS5100.5 (Ref. 3) guidelines, with the area of the gross section Agross = 317 × 103 mm2 and the second moment of area of the gross-section about the centroidal axis Igross = 49,900 × 106 mm4 . The centroid of the gross cross-sectional area is located 602 mm below its top ﬁbre, i.e. dc = 602 mm. The section is subjected to a compressive axial force Ne,0 = −100 kN and a hogging moment of Me,0 = −50 kNm applied with respect to the reference x-axis, that is taken in this example to be 300 mm below the top ﬁbre of the cross-section. All materials are linear-elastic with Ec,0 = 32 GPa and Es = Ep = 200 GPa. The modular ratios of the reinforcing steel and the prestressing steel are therefore ns(i),0 = np(i),0 = 6.25. The prestressing forces applied to the top and bottom tendons (Ap(1) and Ap(2) , respectively) prior to the transfer of prestress are Pp(1),init = Pp(2),init = 1000 kN. The distances of the steel layers from the reference axis are ys(1) = −240 mm, ys(2) = +790 mm, yp(1) = +580 mm and yp(2) = +710 mm. From Eq. 5.5, the initial strains in the prestressing steel layers prior to the transfer of prestress to the concrete are: εp(1),init = εp(2),init =

1000 × 103 = 0.00625 800 × 200 × 103

The vector of external actions at ﬁrst loading is

−100 × 103 N re,0 = −50 × 106 Nmm

148 Uncracked sections As(1) = 900 mm2

ds(1) = 60

dref = 300 dc = 602

x Centroidal axis of precast concrete I-girder

dp(1) = 880

Ap(1) = 800 mm2

dp(2) = 1010 ds(2) = 1090

Ap(2) = 800 mm2 As(2) = 1800 mm2

D = 1150 y

Figure 5.7 Precast prestressed concrete section for Example 5.2 (dimensions in mm).

and, from Eq. 5.13d, the vector of initial prestressing forces is: fp,init =

2 i=1

Ap(i) Ep(i) εp(i),init

yp(i) Ap(i) Ep(i) εp(i),init

800 × 200,000 × 0.00625 800 × 200,000 × 0.00625 + 580 × 800 × 200,000 × 0.00625 710 × 800 × 200,000 × 0.00625 2000 × 103 N = 1290 × 106 Nmm

=

The relevant cross-sectional properties of the transformed section expressed in equivalent concrete areas are: A0 = Agross + (ns,0 − 1)[As(1) + As(2) ] + (np,0 − 1)[Ap(1) + Ap(2) ] = 317 × 103 + (6.25 − 1) × [900 + 1800] + (6.25 − 1) × [800 + 800] = 339.6 × 103 mm2 B0 = Agross (dc − dref ) + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] + (np,0 − 1)[Ap(1) yp(1) + Ap(2) yp(2) ] = 317 × 103 × (602 − 300) + (6.25 − 1) × [900 × (−240) + 1800 × 790] + (6.25 − 1) × [800 × 580 + 800 × 710] = 107.5 × 106 mm3 2 2 I0 = Igross + Agross (dc − dref )2 + (ns,0 − 1)(As(1) ys(1) + As(2) ys(2) ) 2 2 + Ap(2) yp(2) ) = 49,900 × 106 + 317 × 103 + (np,0 − 1)(Ap(1) yp(1)

× (602 − 300)2 + (6.25 − 1) × [900 × (−240)2 + 1800 × 7902 ] + (6.25 − 1) × [800 × 5802 + 800 × 7102 ] = 88,510 × 106 mm4

Uncracked sections 149 From Eq. 5.18: 1 32,000 × (339,600 × 88,510 × 106 − (107.5 × 106 )2 ) 88,510 × 106 −107.5 × 106 × −107.5 × 106 339,600 149.5 × 10−12 N−1 −181.5 × 10−15 N−1 mm−1 = −181.5 × 10−15 N−1 mm−1 573.5 × 10−18 N−1 mm−2

F0 =

The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.14: 149.5 × 10−12 −181.5 × 10−15 ε0 = F0 re,0 − fp,init = −181.5 × 10−15 573.5 × 10−18 ! −100 × 103 2000 × 103 × − −50 × 106 1290 × 106 −70.7 × 10−6 = −0.387 × 10−6 mm−1 The strain at the reference axis and the curvature are therefore εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 and, from Eq. 5.1, the top (y = −300 mm) and bottom (y = +850 mm) ﬁbre strains are: ε0(top) = εr,0 −300×κ0 = (−70.7−300×(−0.387))×10−6 = +45.5×10−6 and ε0(btm) = εr,0 +850×κ0 = (−70.7+850×(−0.387))×10−6 = −399.8×10−6 From Eq. 5.16a, the top and bottom ﬁbre stresses in the concrete are: σc,0(top) = Ec,0 ε0(top) = 32,000 × 45.5 × 10−6 = +1.45 MPa σc,0(btm) = Ec,0 ε0(btm) = 32,000 × (−399.8) × 10−6 = −12.8 MPa and, from Eq. 5.16b, the stresses in the two layers of non-prestressed reinforcement are: −70.7 × 10−6 3 σs(1),0 = 200 × 10 × 1 −240 = 4.5 MPa −0.387 × 10−6 and σs(2),0 = 200 × 10 × 1 790 3

−70.7 × 10−6 = −0.387 × 10−6

−75.3 MPa

150 Uncracked sections The stresses in the two layers of prestressing steel are obtained from Eq. 5.16c: σp(1),0 = Ep 1 yp(1) ε0 + Ep εp(1),init −70.7 × 10−6 3 = 200 × 10 × 1 580 + 200,000 × 0.00625 −0.387 × 10−6 = 1191 MPa and σp(2),0 = Ep 1 yp(2) ε0 + Ep εp(2),init −70.7 × 10−6 3 = 200 × 10 × 1 710 + 200,000 × 0.00625 −0.387 × 10−6 = 1181 MPa. The stress and strain distributions are plotted in Fig. 5.8. +45.5 × 10−6

+1.45 4.5

e

x

s

k0 = −0.387 × 10−6 mm−1

1191 −75.3 −6

−399.8 × 10

y (a) Cross-section

(b) Strain diagram

1181

−12.8 (c) Stress diagram (MPa)

Figure 5.8 Strain and stress diagrams for Example 5.2.

As already outlined in Example 5.1, the cross-sectional rigidities included in F0 can also be calculated based on Eqs 5.9 and 5.11 considering the individual contribution of each component without modifying their geometry (i.e. without transforming the section): RA,0 = Agross Ec,0 + As(1) + As(2) Es − Ec,0 + Ap(1) + Ap(2) Ep − Ec,0 = 10,866 × 106 N RB,0 = Agross dc − dref Ec,0 + As(1) ys(1) + As(2) ys(2) Es − Ec,0 + Ap(1) yp(1) + Ap(2) yp(2) Ep − Ec,0 = 3439 × 109 Nmm 2 2 2 RI,0 = Igross + Agross dc − dref Ec,0 + As(1) ys(1) Es − Ec,0 + As(2) ys(2) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep − Ec,0 = 2832 × 1012 Nmm2

Uncracked sections 151 Matrix F0 can then be determined as (Eq. 5.15): 1

F0 =

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 −181.5 × 10−15 N−1 mm−1 149.5 × 10−12 N−1 = −181.5 × 10−15 N−1 mm−1 573.5 × 10−18 N−1 mm−2

5.4 Long-term analysis of reinforced or prestressed concrete cross-sections using the age-adjusted effective modulus method (AEMM) Cross-sectional analysis using the age-adjusted effective modulus method (see Section 4.4) provides an effective tool for determining how stresses and strains vary with time due to creep and shrinkage of concrete and relaxation of the prestressing steel (if any). For this purpose, two instants in time are identiﬁed, as shown in Fig. 5.9. One time instant is the time at ﬁrst loading, i.e. t = τ0 , and one represents the instant in time at which stresses and strains need to be evaluated, i.e. t = τk . It is usually convenient to measure time in days starting from the time when the concrete is poured. During the time interval tk (= τk − τ0 ), creep and shrinkage strains develop in the concrete and relaxation occurs in the prestressing steel. The gradual change of strain in the concrete with time causes changes of stress in the bonded reinforcement. In general, as the concrete shortens due to compressive creep and shrinkage, the reinforcement is compressed and there is a gradual increase in the compressive stress in the nonprestressed reinforcement and a gradual loss of prestress in any bonded prestressing tendons. To maintain equilibrium, the gradual change of force in the steel at each bonded reinforcement level is opposed by an equal and opposite restraining force on the concrete, as shown in Fig. 5.10. These gradually applied forces (Tc.s(i) and Tc.p(i) ) are usually tensile and, for a prestressed or partially-prestressed cross-section, tend to relieve the concrete of its initial compression. The resultants of the creep and shrinkage-induced internal restraining forces on the concrete are an increment of axial force N(τk ) and an increment of moment about the reference axis M(τk ) given by: N(τk ) =

ms i=1

Tc.s(i) +

mp

Tc.p(i)

(5.19a)

i=1

and M(τk ) =

ms i=1

Tc.s(i) ys(i) +

mp

Tc.p(i) yp(i)

(5.19b)

i=1

Equal and opposite actions −N(τk ) and −M(τk ) are applied to the bonded steel parts of the cross-section.

152 Uncracked sections Duration of load, Dtk =tk−t0 t=0

t0

tk

Concrete pour

First loading

Time instant at which stresses and deformations are sought

Time, t

Figure 5.9 Relevant instants in time (AEMM). erk DTc.s(1)

ys(1)

Der

x ys(2) yp(2)

yp(1)

kk DTc.p(1) DTc.p(2) DTc.s(2)

y Section

Elevation

time, tk

Restraining forces

er0 k0 t0

Strain

Figure 5.10 Time-dependent actions and deformations.

The strain at any depth y below the reference axis at time τk may be expressed in terms of the strain at the reference axis εrk and the curvature κk : εk = εr,k + yκk

(5.20)

The magnitude of the change of strain that occurs with time εk (= εk − ε0 ) is the sum of each of the following components: (a) the free shrinkage strain εsh (τk ) (which is usually considered to be uniform over the section); (b) the unrestrained creep strain caused by the initial concrete stress σc,0 existing at the beginning of the time period, i.e. εcr,k = ϕ(τk , τ0 )σc,0 /Ec,0 ; and (c) the creep and elastic strain caused by N(τk ) and M(τk ) gradually applied to the concrete cross-section throughout the time period. For the time analysis, the steel reinforcement and prestressing tendons (if any) are assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationship for the concrete is that given by Eq. 4.45. The stress-strain relationships for each material at τ0 and at τk are as follows. At τ0 : σc,0 = Ec,0 ε0 σs(i),0 = Es(i) ε0 σp(i) = Ep(i) ε0 + εp(i),init

(5.21a) (5.21b) (5.21c)

Uncracked sections 153 At τk : Fe,0 σc,0 Ee,k εk − εsh,k + σc,k = σs(i),k = Es(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(5.22a) (5.22b) (5.22c)

Ee,k is the age-adjusted effective modulus at t = τk where Fe,0 is given by Eq. 4.46, (Eq. 4.35), and εp.rel(i),k is the tensile creep strain that has developed in the i-th prestressing tendon at time τk (often referred to as the relaxation strain) and may be calculated from: εp.rel(i),k =

Pp(i),init ϕp (τk , σp(i),init ) = εp(i),init ϕp (τk , σp(i),init ) Ap(i) Ep(i)

(5.23a)

where ϕp (τk , σp(i),init ) is the creep coefﬁcient for the prestressing steel at time τk due to an initial stress σp(i),init in the i-th prestressing tendon just prior to transfer (as given in Table 2.7). Alternatively, εp.rel(i),k may be calculated from the relaxation R given in Eq. 2.11 or included in Table 2.7 as: εp.rel(i),k = εp(i),init R

(5.23b)

The governing equations describing the long-term behaviour of a cross-section are obtained by enforcing equilibrium at the cross-section at time τk following the approach already presented in the previous section for the instantaneous analysis at time τ0 (Eqs 5.4–5.18), and by extending the approach outlined for axially loaded uncracked cross-sections in Sections 4.4.1 and 4.4.4. Restating the equilibrium equations (Eqs 5.2) at time τk gives: re,k = ri,k

(5.24)

where

Ne,k Me,k

re,k =

(5.25a)

and

Ni,k ri,k = Mi,k

(5.25b)

Ni,k and Mi,k depict the internal axial force and moment resisted by the cross-section at time τk , while Ne,k and Me,k represent the external applied loads at this time. As in Eq. 5.6, the axial force Ni,k is the sum of the axial forces carried by the concrete, the reinforcement and the tendons: Ni,k = Nc,k + Ns,k + Np,k

(5.26)

154 Uncracked sections Considering the time-dependent constitutive relationship for the concrete (Eq. 5.22a), the axial force resisted by the concrete at time τk can be expressed as: Nc,k = σc,k dA = Ee,k εr,k + yκk − εsh,k + Fe,0 σc,0 d A Ac

Ac

= Ac Ee,k εr,k + Bc Ee,k κk − Ac Ee,k εsh,k + Fe,0 Nc,0

(5.27)

where εr,k and κk are the strain at the level of the reference axis and the curvature at time τk , while Nc,0 is the axial force resisted by the concrete at time τ0 . For the time analysis, Nc,0 is assumed to be known having been determined during the instantaneous analysis from Eq. 5.7a. Using the constitutive equations for the steel (Eqs 5.22b and c), the axial forces carried by the reinforcing bars and the prestressing steel at time τk are calculated as: ms ms Ns,k = As(i) Es(i) εr,k + ys(i) As(i) Es(i) κk i=1

Np,k =

(5.28a)

i=1

mp mp Ap(i) Ep(i) εr,k + yp(i) Ap(i) Ep(i) κk i=1

i=1

mp

+

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.28b)

i=1

By substituting Eqs 5.27 and 5.28 into Eq. 5.26, the internal axial force is given by: mp ms ms As(i) Es(i) + Ap(i) Ep(i) εr,k + Bc Ee,k + ys(i) As(i) Es(i) Ni,k = Ac Ee,k + i=1 mp

+

i=1

i=1

yp(i) Ap(i) Ep(i) κk − Ac Ee,k εsh,k + Fe,0 Nc,0

i=1

+

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

= RA,k εr,k + RB,k κk − Ac Ee,k εsh,k + Fe,0 Nc,0 +

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.29)

i=1

where the axial rigidity and the stiffness related to the ﬁrst moment of area calculated at time τk have been referred to as RA,k and RB,k , respectively, and are given by: Ee,k + RA,k = Ac

ms i=1

RB,k = Bc Ee,k +

ms i=1

As(i) Es(i) +

mp

Ap(i) Ep(i)

(5.30a)

i=1

ys(i) As(i) Es(i) +

mp i=1

yp(i) Ap(i) Ep(i)

(5.30b)

Uncracked sections 155 In a similar manner, the internal moment Mi,k resisted by the cross-section at time τk can be expressed as: mp ms ys(i) As(i) Es(i) + yp(i) Ap(i) Ep(i) εr,k Mi,k = Bc Ee,k + i=1

+ Ic Ee,k +

ms

i=1 2 ys(i) As(i) Es(i) +

i=1

+ Fe,0 Mc,0 +

mp

2 yp(i) Ap(i) Ep(i) κk − Bc Ee,k εsh,k

i=1

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

= RB,k εr,k + RI,k κk − Bc Ee,k εsh,k + Fe,0 Mc,0 +

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.31)

i=1

where the ﬂexural rigidity of the cross-section calculated at time τk , referred to as RI,k in Eq. 5.31, is given by: Ee,k + RI,k = Ic

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

(5.32)

i=1

and Mc,0 is the moment resisted by the concrete component at time τ0 and from the instantaneous analysis: yσc,0 dA = yEc,0 εr,0 + yκ0 dA = Bc Ec,0 εr,0 + Ic Ec,0 κ0 (5.33) Mc,0 = Ac

Ac

After substituting Eqs 5.29 and 5.31 into Eq. 5.24, the equilibrium equations at time τk may be written in compact form as: re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k

(5.34)

where

ε εk = r,k κk

and Dk =

RA,k RB,k RB,k RI,k

(5.35a)

(5.35b)

The vector f cr,k represents the creep effect produced by the stress σc,0 resisted by the concrete at time τ0 and is given by:

Nc,0 Ac εr,0 + Bc κ0 = Fe,0 Ec,0 (5.36) Fe,0 fcr,k = Mc,0 Bc εr,0 + Ic κ0

156 Uncracked sections and Fe,0 is given in Eq. 4.46. The vector f sh,k accounts for the uniform shrinkage strain that develops in the concrete over the time period and is given by: fsh,k =

Ac E ε Bc e,k sh,k

(5.37)

The vector f p,init in Eq. 5.34 accounts for the initial prestress and the vector f p.rel,k accounts for the resultant actions caused by the loss of prestress in the tendon due to relaxation. These are given by: fp,init =

mp Ap(i) Ep(i) εp(i),init yp(i) Ap(i) Ep(i) εp(i),init

(5.38a)

i=1

and fp.rel,k = fp,init ϕp (τk , σp(i),init )

(5.38b)

Eq. 5.34 can be solved for εk as: re,k − fcr,k + fsh,k − fp,init + fp.rel,k εk = D−1 k = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(5.39)

where Fk =

1 RA,k RI,k − R2B,k

RI,k −RB,k −RB,k RA,k

The stress distribution at time τk can then be calculated as follows: " # σc,k = Fe,0 σc,0 = Fe,0 σc,0 Ee,k εk − εsh,k + Ee,k 1 y εk − εsh,k + σs,k(i) = Es(i) εk = Es(i) 1 ys(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(5.40)

(5.41a) (5.41b)

(5.41c)

where at any point y from the reference axis εk = εr,k + yκk = 1 y εk . The cross-sectional rigidities RA,k , RB,k and RI,k , required for the solution at time τk can also be calculated from the properties of the age-adjusted transformed section, obtained by transforming the bonded steel areas (reinforcement and tendons) into equivalent areas of the aged concrete at time τk , as follows: Ak Ee,k RA,k =

(5.42a)

RB,k = Bk Ee,k

(5.42b)

RI,k = I¯k Ee,k

(5.42c)

Uncracked sections 157 where Ee,k is the age-adjusted effective modulus, Ak is the area of the age-adjusted transformed section, and Bk and I¯k are the ﬁrst and second moments of the area of the age-adjusted transformed section about the reference axis. For the determination of Ak , Bk and I¯k , the areas of the bonded steel are transformed into equivalent areas of concrete by multiplying by the age-adjusted modular ratio n¯ es(i),k (= Es(i) /Ee,k ) or n¯ ep(i),k = (Ep(i) /Ee,k ), as appropriate. Based on Eqs 5.42, the expression for Fk (Eq. 5.40) can be re-written as: I¯k − Bk 1 Fk = Ee,k ( Ak I¯k − B2k ) − Ak Bk

(5.43)

The calculation of the time-dependent stresses and deformations using the above procedure is illustrated in Examples 5.3 and 5.4.

Example 5.3 For the reinforced concrete section shown in Fig. 5.5, the strain and stress distributions at τ0 immediately after the application of an axial force Ne,0 = −30 kN and a bending moment of Me,0 = 50 kNm were calculated in Example 5.1. If the applied loads remain constant during the time interval τ0 to τk , the strain and stress distributions at time τk are to be determined using the age-adjusted effective modulus method. As in Example 5.1, Ec,0 = 25 GPa; Es = 200 GPa; and ns,0 = Es /Ec,0 = 8. Take ϕ (τk , τ0 ) = 2.5; χ (τk , τ0 ) = 0.65; εsh (τk ) = −600 × 10−6 and assume the steel reinforcement is linear elastic. From Example 5.1: At τ0 : εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 25,000 = 9524 MPa = 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.5

and therefore n¯ es,k = 21.0; ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.5 × (0.65 − 1.0) = −0.333 Fe,0 = = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.5 The properties of the concrete part of the cross-section are: Ac = bD − As(1) − As(2) = 300 × 600 − 620 − 1800 = 177,600 mm2 Bc = bD(D/2 − dref ) − As(1) ys(1) − As(2) ys(2) = 300 × 600 × (300 − 200) − 620 × (−150) − 1800 × 350 = 17.46 × 106 mm3

2 bD3 D 300 × 6003 2 2 Ic = + bD − dref − As(1) ys(1) − As(2) ys(2) = 12 2 12 + 300 × 600 × (300 − 200)2 − 620 × (−150)2 − 1800 × 3502 = 6966 × 106 mm4

158 Uncracked sections and the properties of the age-adjusted transformed cross-section are: Ak = bD + (n¯ es,k − 1)[As(1) + As(2) ] = 300 × 600 + (21 − 1) × [620 + 1800] = 228,400 mm2

D Bk = bD − dref + (n¯ es,k − 1)[As(1) ys(1) + As(2) ys(2) ] = 300 × 600 2 × (300 − 200) + (21 − 1) × [620 × (−150) + 1800 × 350] = 28.74 × 106 mm3

2 3 ¯Ik = bD + bD D − dref + (n¯ es,k − 1)[As(1) y2 + As(2) y2 ] s(1) s(2) 12 2 300 × 6003 + 300 × 600 × (300 − 200)2 + 20 × [620 × (−150)2 12

=

+ 1800 × 3502 ] = 11,890 × 106 mm4 From Eq. 5.36: ⎤ ⎡ 177,600 × −42.7 × 10−6 + 17.46 × 106 ⎥ ⎢ ×0.331 × 10−6 ⎥ ⎢ fcr.k = −0.333 × 25,000 × ⎢ ⎥ ⎣17.46 × 106 × −42.7 × 10−6 + 6966 × 106 ⎦ ×0.331 × 10−6 =

+14.9 × 103 N

−13.0 × 106 Nmm

and from Eq. 5.37: 177,600 × 9524 × −600 × 10−6 −1015 × 103 N = fsh,k = −99.79 × 106 Nmm 17.46 × 106 × 9524 × −600 × 10−6

Eq. 5.43 gives: Fk =

1 9524 × (228,400 × 11,890 × 106 − (28.74 × 106 )2 ) 11,890 × 106 −28.74 × 106 × −28.74 × 106 228,400

=

660.7 × 10−12 N−1

−1.597 × 10−12 N−1 mm−1

−1.597 × 10−12 N−1 mm−1

12.69 × 10−15 N−1 mm−2

Uncracked sections 159 The strain εk at time τk is determined using Eq. 5.39: εk = Fk (re,k − fcr,k + fsh,k ) 660.7 × 10−12 −1.597 × 10−12 (−30 − 14.9 − 1015) × 103 = −1.597 × 10−12 12.69 × 10−15 (50 + 13.0 − 99.79) × 106 −641.4 × 10−6 = +1.226 × 10−6 mm−1 That is, the strain at the reference axis and the curvature at time τk are εr,k = −641.4 × 10−6 and κk = +1.226 × 10−6 mm−1 , respectively, and from Eq. 5.1, the top (y = −200 mm) and bottom (y = +400 mm) ﬁbre strains are: εk(top) = εr,k + (−200) × κk = (−641.4 − 200 × 1.226) × 10−6 = −886.5 × 10−6 and εk(btm) = εr,k +400×κk = (−641.4+400×1.226)×10−6 = −151.1×10−6 The concrete stress distribution at time τk is calculated using Eq. 5.41a: σc,k(top) = 9524

! −641.4 × 10−6 −6 1 −200 − (−600 × 10 ) +1.226 × 10−6

+ (−0.333) (−2.27) = −1.82 MPa ! −641.4 × 10−6 −6 σc,k(btm) = 9524 1 400 − (−600 × 10 ) +1.226 × 10−6 + (−0.333) (2.25) = 3.52 MPa and, from Eq. 5.42b, the stresses in the reinforcement are:

−641.4 × 10−6 +1.226 × 10−6

3

1 −150

3

−641.4 × 10−6 1 350 +1.226 × 10−6

σs(1),k = Es(1) 1 ys(1) εk = 200 × 10 = −165 MPa and

σs(2),k = Es(2) 1 ys(2) εk = 200 × 10 = −42.5 MPa

160 Uncracked sections The stress and strain distributions at τo (from Example 5.1) and at τk are shown in Fig. 5.11. time, t0 time, tk −886.5

−2.72 −1.82 −165 −18.5

−108.9

x

σ

e 0.331 × 10 −6

1.226 × 10

−6

mm

−1

mm

−42.5 14.6 −151.1

y

89.8

(b) Strain (× 10−6)

(a) Cross-section

−1

2.25 3.52 (c) Stress (MPa)

Figure 5.11 Strain and stress diagrams for Example 5.3 (all units in mm, MPa).

The cross-sectional rigidities could also have been calculated based on Eqs 5.30 and 5.32 without modifying the geometry of the section as: Ee,k + RA,k = Ac

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) = Ac Ec0 + As(1) + As(2) Es

i=1

6

= 2175 × 10 N; Ee,k + RB,k = Bc

ms

ys(i) As(i) Es(i) +

mp

i=1

yp(i) Ap(i) Ep(i)

i=1

= Bc Ee,k + As(1) ys(1) + As(2) ys(2) Es = 273.7 × 109 Nmm; and Ee,k + RI,k = Ic

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

i=1

2 2 = Ic Ee,k + As(1) ys(1) + As(2) ys(2) Es = 113.2 × 1012 Nmm2 . Fk is then determined using Eq. 5.40 (and is identical to that calculated earlier using Eq. 5.43):

RI,k −RB,k 1 Fk = RA,k RI,k − R2B,k −RB,k RA,k =

1

2 273.7 × 109 −273.7 × 109 2175 × 106

2175 × 106 × 113.2 × 1012 −

×

113.2 × 1012 −273.7 × 109

660.7 × 10−12 N−1 −1.597 × 10−12 N−1 mm−1 = −1.597 × 10−12 N−1 mm−1 12.69 × 10−15 N−1 mm−2

Uncracked sections 161

Example 5.4 A time-dependent analysis of the prestressed concrete section of Example 5.2 (see Figure 5.7) is to be undertaken using the age-adjusted effective modulus method. The strain and stress distributions at τ0 immediately after the application of an axial force Ne,0 = −100 kN and a bending moment of Me,0 = −50 kNm were calculated in Example 5.2. If the applied loads remain constant during the time interval τ0 to τk , the strain and stress distributions at time τk are to be determined. As in Example 5.2: Ec,0 = 32 GPa; Es = Ep = 200 GPa; and therefore ns(i),0 = np(i),0 = 6.25. Take ϕ(τk , τ0 ) = 2.0; χ(τk , τ0 ) = 0.65; εsh (τk ) = −400 × 10−6 and, for the prestressing steel, ϕp (τk , τ0 , σp(i),init ) = 0.03. Assume the steel reinforcement is linear elastic. From Example 5.2 at τ0 : εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

32,000 = 13,910 MPa and therefore n¯ es,k = n¯ ep,k = 14.37 1 + 0.65 × 2.0

2.0 × (0.65 − 1.0) Fe,0 = = −0.304 1.0 + 0.65 × 2.0 The properties of the concrete part of the cross-section are: Ac = Agross − As(1) − As(2) − Ap(1) − Ap(2) = 312,700 mm2 Bc = Agross (dc − dref ) − [As(1) ys(1) + As(2) ys(2) ] − [Ap(1) yp(1) + Ap(2) yp(2) ] = 93.49 × 106 mm3 2 2 2 Ic = Igross + Agross (dc − dref )2 − [As(1) ys(1) + As(2) ys(2) ] − [Ap(1) yp(1) 2 + Ap(1) yp(1) ] = 76,960 × 106 mm4

and the properties of the age-adjusted transformed section in equivalent concrete areas are: Ak = Agross + (n¯ es,k − 1)[As(1) + As(2) ] + (n¯ ep,k − 1)[Ap(1) + Ap(2) ] = 374.5 × 103 mm2 Bk = Agross (dc − dref ) + (n¯ es,k − 1)[As(1) ys(1) + As(2) ys(2) ] + (n¯ ep,k − 1)[Ap(1) yp(1) + Ap(2) yp(2) ] = 125.7 × 106 mm3 2 2 I¯k = Igross + Agross (dc − dref )2 + (n¯ es,k − 1)(As(1) ys(1) + As(2) ys(2) ) 2 2 + Ap(2) yp(2) ) = 103.5 × 109 mm4 + (n¯ ep,k − 1)(Ap(1) yp(1)

162 Uncracked sections Eqs 5.36 and 5.37 give: +567.9 × 103 N fcr.k = +354.6 × 106 Nmm

and −1740 × 103 N fsh,k = −520 × 106 Nmm

and from Eq. 5.38a (and Example 5.2) and Eq. 5.38b: fp,init =

2000 × 103 N

1290 × 106 Nmm

and fp.rel,k =

2000 × 103 × 0.03

1290 × 106 × 0.03

=

60 × 103 N

38.7 × 106 Nmm

Using Eq. 5.43:

−393.1 × 10−15 N−1 mm−1 323.8 × 10−12 N−1 Fk = −393.1 × 10−15 N−1 mm−1 1.171 × 10−15 N−1 mm−2

and the strain vector εk at time τk is determined using Eq. 5.39: 323.8 × 10−12 −393.1 × 10−15 εk = −393.1 × 10−15 1.171 × 10−15 (−100 − 567.9 − 1740 − 2000 + 60) × 103 × (−50 − 354.6 − 520 − 1290 + 38.7) × 106 −552.5 × 10−6 = −0.840 × 10−6 mm−1

The strain at the reference axis and the curvature at time τk are therefore εr,k = −552.5 × 10−6 and κk = −0.840 × 10−6 mm−1 , respectively. From Eq. 5.1, the top (y = −300 mm) and bottom (y = +850 mm) ﬁbre strains are: εk(top) = εr,k + (−300) × κk = −300.5 × 10−6 and εk(btm) = εr,k + 850 × κk = −1266 × 10−6

Uncracked sections 163 The concrete stress distribution at time τk is calculated using Eq. 5.41a: ! −552.5 × 10−6 −6 σc,k(top) = 13,913 1 −300 − (−400 × 10 ) −0.840 × 10−6 + (−0.304) (1.45) = 0.94 MPa ! −552.5 × 10−6 −6 σc,k(btm) = 13,913 1 850 − (−400 × 10 ) −0.840 × 10−6 + (−0.304) (−12.8) = −8.16 MPa and, from Eq. 5.41b, the stresses in the non-prestressed reinforcement are: −552.5 × 10−6 3 σs(1),k = Es(1) 1 ys(1) εk = 200 × 10 1 −240 −0.840 × 10−6 = −70.2 MPa and

3

σs(2),k = Es(2) 1 ys(2) εk = 200 × 10

−552.5 × 10−6 1 790 −0.840 × 10−6

= −243.3 MPa From Example 5.2, the initial strains in the prestress before transfer are εp(1),init = εp(2),init = 0.00625 and the relaxation strains are therefore εp.rel(1),k = εp.rel(2),k = 0.00625 × 0.03 = 187.5 × 10−6 . The stresses in the prestressing tendons at τk are obtained from Eq. 5.41c: −552.5 × 10−6 σp(1),k = 200,000 × [1 580] + 0.00625 − 0.0001875 −0.840 × 10−6 = 1004 MPa and

−552.5 × 10−6 σp(2),k = 200,000 × [1 710] + 0.00625 − 0.0001875 −0.840 × 10−6 = 982 MPa

The changes in stress in each prestressing tendon between ﬁrst loading and time τk are therefore σp(1),k = σp(1),0 −σp(1),k = 1191−1004 = 187 MPa and σp(2),k = σp(2),0 − σp(2),k = 1181 − 982 = 199 MPa and represent the time-dependent loss of prestress in each tendon, with σp(1),k being 15.7 per cent of the initial stress in Ap(1) immediately after transfer and σp(2),k being 16.8 per cent of the initial stress in Ap(2) .

164 Uncracked sections The stress and strain distributions at τ0 (from Example 5.2) and at τk are shown in Fig. 5.12. −300.5 45.5

0.94 + 1.45 4.5 s

kk = −0.840 × 10−6 mm−1

x

−70.2 e

Time, t0 Time, tk k0 = −0.387 × 10−6 mm−1 −243.3

−1266 −399.8 y (a) Cross-section (b) Strain diagram (× 10−6)

−75.3

1191 1004 1181 982

−12.8 −8.16 (c) Stress diagram (MPa)

Figure 5.12 Strain and stress distributions for Example 5.4.

The cross-sectional rigidities calculated using Eqs 5.30 and 5.32 are: RA,k = Ac Ee,k + As(1) + As(2) Es + Ap(1) + Ap(2) Ep = 5210 × 106 N RB,k = Bc Ee,k + As(1) ys(1) + As(2) ys(2) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 1748 × 109 Nmm 2 2 RI,k = Ic Ee,k + As(1) ys(1) Es + As(2) ys(2) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 1440 × 1012 Nmm2 and the matrix Fk could have been determined conveniently using Eq. 5.41.

5.5 Long-term analysis of reinforced and prestressed cross-sections using the step-by-step procedure The age-adjusted effective modulus method outlined in the previous section is a practical means to evaluate the time-dependent deformations and stresses on a reinforced or prestressed concrete section. It involves a single time interval, with stresses and deformations calculated at the beginning and end of the time interval, i.e. at τ0 and τk as shown in Fig. 5.9. The level of accuracy of the results depends on the type of stress and/or deformation history undergone by the concrete. For a more accurate representation of concrete behaviour, a more reﬁned method may be required, such as the step-by-step method (see Section 4.3) or the Dirichlet Series approximation (Ref. 4–5). The step-by-step procedure involves the time domain being discretised into a number of instants τj (with j = 0, . . . , k), as shown in Fig. 4.3, with the latter instant in time τk being the one at which the structural response is sought. Structural response is calculated at each time instant, in turn, with the solution at τj relying on the solutions obtained at the previous time instants. To achieve this, the concrete stresses calculated at each instant in time are stored for use in the subsequent analyses.

Uncracked sections 165 The steel reinforcement and prestressing tendons (if any) are again assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationships for the steel at any time τj are: σs(i),j = Es(i) εj σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j

(5.44a) (5.44b)

Following the approach outlined in Section 4.3.3, the constitutive relationship for the concrete at τj is given by Eq. 4.25 reproduced below: j−1

σc,j = Ec,j εj − εsh,j + Fe,j,i σc,i

(4.25)

i=0

and if the rectangular approximation of the integral-type creep law is adopted, the instantaneous elastic modulus of concrete Ec,j and the term Fe,j,i are given by Eqs 4.26a and b (reproduced below for ease of reference): Ec,j =

1 Jj,j

(4.26a)

and Fe,j,i =

Jj,i+1 − Jj,i Jj,j

(4.26b)

If the trapezoidal approximation is used for the numerical integration, the expressions for Ec,j and Fe,j,i are given in Eqs 4.26c–f. For ease of notation, the rectangular rule is considered in this chapter and used in the subsequent examples. With the proposed approach, k + 1 analyses must be carried out in order to yield the structural response at any time τk . For each time instant τj (with j = 0, . . . , k), the equations utilised in the cross-sectional analysis are obtained from considerations of equilibrium: ri,j = re,j

(5.45)

where ri,j and re,j are, respectively, the internal cross-sectional stress resultants and the external actions calculated at time τj , as follows:

Ni,j ri,j = Mi,j

(5.46a)

and

Ne,j re,j = Me,j

(5.46b)

where Ni,j and Mi,j depict the internal axial force and moment resisted by the crosssection at time τj , while Ne,j and Me,j represent the external applied actions.

166 Uncracked sections As already presented for the AEMM, the internal actions can be calculated by combining the contributions of the concrete, reinforcing steel and tendons. For example, the internal axial force resisted by the cross-section at τj can be expressed as: Ni,j = Nc,j + Ns,j + Np,j

(5.47)

The axial force in the concrete can be represented based on its constitutive relationship (Eq. 4.25) as: ⎡ ⎤ j−1 ⎣Ec,j εj − εsh,j + σc,j dA = Fe,j,i σc,i ⎦ dA Nc,j = Ac

Ac

i=0

= Ac Ec,j εr,j + Bc Ec,j κj − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

(5.48)

i=0

where the axial forces Nc,i resisted by the concrete at times τi (with i = 0, . . . , j − 1) are known (i.e. they have been calculated in previous time steps) at the beginning of the analysis at τj . The axial forces in the reinforcement and tendons can be evaluated from the constitutive relations (Eqs 5.44) as: Ns,j =

ms ms As(i) Es(i) εr,j + ys(i) As(i) Es(i) κj i=1

(5.49a)

i=1

mp

Np,j =

mp Ap(i) Ep(i) εr,j + yp(i) Ap(i) Ep(i) κj i=1

+

i=1

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.49b)

i=1

Substituting Eqs 5.48 and 5.49 into Eq. 5.47 produces: mp ms ms As(i) Es(i) + Ap(i) Ep(i) εr,j + Bc Ec,j + ys(i) As(i) Es(i) Ni,j = Ac Ec,j + i=1 mp

+

i=1

i=1

yp(i) Ap(i) Ep(i) κj − Ac Ec,j εsh,j +

i=1

+

mp

j−1

Fe,j,i Nc,i

i=0

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

i=1

= RA,j εr,j + RB,j κj − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

i=0

+

mp i=1

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.50)

Uncracked sections 167 and following the same procedure, the internal moment Mi,j at τj can be determined as: Mi,j = Bc Ec,j +

ms

ys(i) As(i) Es(i) +

i=1

j−1

yp(i) Ap(i) Ep(i) εr,j

mp

2 ys(i) As(i) Es(i) +

i=1

+

i=1

ms

+ Ic Ec,j +

mp

2 yp(i) Ap(i) Ep(i)

κj − Bc Ec,j εsh,j

i=1

Fe,j,i Mc,i +

i=0

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

i=1

= RB,j εr,j + RI,j κj − Bc Ec,j εsh,j +

j−1

Fe,j,i Mc,i

i=0

+

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.51)

i=1

The cross-sectional rigidities RA,j , RB,j and RI,j at time τj are deﬁned as: RA,j = Ac Ec,j +

ms

As(i) Es(i) +

i=1

RB,j = Bc Ec,j +

RI,j = Ic Ec,j +

ms

mp

Ap(i) Ep(i)

(5.52a)

i=1

ys(i) As(i) Es(i) +

mp

i=1

i=1

ms

mp

2 ys(i) As(i) Es(i) +

i=1

yp(i) Ap(i) Ep(i)

2 yp(i) Ap(i) Ep(i)

(5.52b)

(5.52c)

i=1

In the calculation of Mi,j in Eq. 5.51, the moment Mc,i resisted by the concrete component at time τi is calculated based on the solutions at each of the previous time instants: Mc,i =

Ac

yσc,i dA =

Ac

i−1 yEc,i εi − εsh,i + y Fe,i,n σc,n dA

= Bc Ec,i εr,i + Ic Ec,i κi − Bc Ec,i εsh,i +

n=0 i−1

Fe,i,n Mc,n

(5.53)

n=0

Following the approach outlined previously, the equilibrium equations at time τj can then be written as: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j

(5.54)

168 Uncracked sections where

εr,j εj = κj

RA,j RB,j Dj = RB,j RI,j fcr,j =

j−1

(5.55a) (5.55b)

Fe,j,i rc,i

(5.55c)

i=0

fsh,j = fp,init =

Ac Ec,j εsh,j Bc mp Ap(i) Ep(i) εp(i),init

(5.55d)

(5.55e)

yp(i) Ap(i) Ep(i) εp(i),init

i=1

fp.rel,j = fp,init ϕp (τj , σp(i),init )

(5.55f)

To simplify the notation, the internal actions resisted by the concrete at a previous time instant τi (calculated from Eqs 5.48 and 5.53) are collected in vector rc,i and expressed as:

i−1 Nc,i Ac Ec,i rc,i = = Dc,i εi + Fe,i,n rc,n − ε = Dc,i εi + fcr,i − fsh,i Mc,i Bc Ec,i sh,i

(5.56)

n=0

with

Ac Bc Dc,i = Ec,i Bc Ic

(5.57)

The strain vector εj at time τj is obtained by solving Eq. 5.54 and, as in the analyses presented earlier: εj = D−1 re,j − fcr,j + fsh,j − fp,init + fp.rel,j = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j j (5.58) in which Fj =

1 RA,j RI,j − R2B,j

RI,j −RB,j −RB,j RA,j

(5.59)

Finally, the stress distributions at time, τj , can be determined from the constitutive relationships (Eqs 5.44 and 4.25): σc,j = Ec,j εj − Ec,j εsh,j +

j−1 i=0

j−1

Fe,j,i σc,i = Ec,j

& ' 1 y εj − εsh,j + Fe,j,i σc,i i=0

(5.60a)

Uncracked sections 169

σs(i),j = Es(i) εj = Es(i) 1 yp(i) εj σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j = Ep(i) 1 yp(i) εj + Ep(i) εp(i),init − Ep(i) εp.rel(i),j

(5.60b)

(5.60c)

where εj = εr,j + yκj = 1 y εj . The cross-sectional rigidities at time τj , RA,j , RB,j and RI,j , can also be calculated from the properties of the transformed cross-section as follows: RA,j = Aj Ee,j

(5.61a)

RB,j = Bj Ee,j

(5.61b)

RI,j = Ij Ee,j

(5.61c)

where Aj , Bj and Ij are the area and the ﬁrst and second moments of the area, respectively, of the transformed section about the reference axis. For the transformed section, the area of the reinforcement and bonded tendons are usually transformed into equivalent areas of concrete, based on Ec,j using modular ratios of ns(i),j (= Es(i) /Ec,j ) for the bonded steel reinforcement and np(i),j (= Ep(i) /Ec,j ) for the bonded tendons. The matrix F0 in Eq. 5.58 can then be calculated as:

Ij Fj = 2 −B Ee,j (Aj Ij − Bj ) j 1

−Bj Aj

(5.62)

In the following two examples, Examples 5.3 and 5.4 are re-analysed using the step-by-step method.

Example 5.5 For the reinforced concrete section shown in Fig. 5.5 (and analysed previously in Examples 5.1 and 5.3), determine the stress distribution at 30,000 days after ﬁrst loading (i.e. approx. 80 years) using the step-by-step procedure. The external loading is applied at time τ0 = 28 days and kept constant over time (i.e. Ne,j = −30 kN and Me,j = 50 kNm). A very coarse time discretisation is adopted in this example to illustrate all the steps involved in the solution process. The time period is subdivided into two intervals, τ0 to τ1 and τ1 to τ2 , where τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. In structural design, a ﬁner discretisation is usually adopted to obtain more accurate results. For convenience in this example, shrinkage is assumed to begin at the time of ﬁrst loading (i.e. at τ0 ). The reinforcement is assumed to be linear-elastic. The relevant properties of the concrete are as follows: Ec,0 = 25 GPa; Ec,1 = 28 GPa; Ec,2 = 30 GPa; ϕ (τ0 , τ0 ) = 0; ϕ (τ1 , τ0 ) = 1.5; ϕ (τ2 , τ0 ) = 2.5; ϕ (τ1 , τ1 ) = 0; ϕ (τ2 , τ1 ) = 2.0; εsh (τ0 ) = εsh,0 = 0; εsh (τ1 ) = εsh,1 = −300 × 10−6 ; and εsh (τ2 ) = εsh,2 = −600 × 10−6 .

170 Uncracked sections Usually when using the step-by-step method (SSM), it is convenient to calculate the material properties for the concrete at the beginning of the analysis. From Eqs 1.10 and 4.26a and b: J (τ0 , τ0 ) =

1 1 = = 4 × 10−5 MPa−1 Ec,0 25,000

J (τ1 , τ1 ) =

1 1 = = 3.571 × 10−5 MPa−1 Ec,1 28,000

J (τ2 , τ2 ) =

1 1 = = 3.333 × 10−5 MPa−1 Ec,2 30,000

J (τ1 , τ0 ) =

1 + ϕ (τ1 , τ0 ) 1 + 1.5 = = 10 × 10−5 MPa−1 Ec,0 25,000

J (τ2 , τ0 ) =

1 + ϕ (τ2 , τ0 ) 1 + 2.5 = = 14 × 10−5 MPa−1 Ec,0 25,000

J (τ2 , τ1 ) =

1 + ϕ (τ2 , τ1 ) 1 + 2.0 = = 10.71 × 10−5 MPa−1 Ec,1 28,000

Fe,1,0 =

J (τ1 , τ1 ) − J (τ1 , τ0 ) = −1.8 J (τ1 , τ1 )

Fe,2,0 =

J (τ2 , τ1 ) − J (τ2 , τ0 ) = −0.986 J (τ2 , τ2 )

Fe,2,1 =

J (τ2 , τ2 ) − J (τ2 , τ1 ) = −2.214 J (τ2 , τ2 )

Considering that the externally applied actions remain constant with time and the problem involves no prestressing tendons (for j = 0, 1 and 2):

−30 × 103 N re,j = 50 × 106 Nmm

0N fp,init = 0 Nmm

0N fp.rel,j = 0 Nmm

Short-term analysis (τ0 = 28 days) From Example 5.1: εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 . From Example 5.3: Ac = 177.6 × 103 mm2 , Bc = 17.46 × 106 mm3 and Ic = 6966 × 106 mm4 .

Uncracked sections 171 The stress resultants resisted by the concrete at τ0 are determined from Eq. 5.56: rc,0 = Dc,0 ε0 + fcr,0 − fsh,0 177.6 × 103 17.46 × 106 −42.7 × 10−6 0 0 = 25,000 × + − −6 6 6 0 0 0.331 × 10 17.46 × 10 6966 × 10 −44.9 × 103 N = 39.1 × 106 Nmm

Time analysis – SSM (τ1 = 100 days) – time step 1: Considering Ec,1 for the concrete component, the cross-sectional rigidities at time τ1 can be determined from Eqs 5.52 as: RA,1 = 5456 × 106 N RB,1 = 596.4 × 109 Nmm RI,1 = 241.9 × 1012 Nmm2 from which D1 and F1 can be determined (Eqs 5.55b and 5.59) as:

5456 × 106 N 596.4 × 109 Nmm RA,1 RB,1 D1 = = RB,1 RI,1 596.4 × 109 Nmm 241.9 × 1012 Nmm2 and F1 =

1

RI,1 −RB,1 −RB,1 RA,1

RA,1 RI,1 − R2B,1 −618.4 × 10−15 N−1 mm−1 250.8 × 10−12 N−1 = −618.4 × 10−15 N−1 mm−1 5.658 × 10−15 N−1 mm−2

Creep effects due to the initial concrete stresses and shrinkage effects are obtained from Eq. 5.55c and d: 80.8 × 103 N −44.9 × 103 fcr,1 = Fe,1,0 rc,0 = −1.8 × = 39.1 × 106 −70.3 × 106 Nmm and

Ac 177.6 × 103 fsh,1 = Ec,1 εsh,1 = × 28,000 × −300 × 10−6 6 Bc 17.46 × 10 −1492 × 103 N = −146.7 × 106 Nmm

172 Uncracked sections The strain distribution at time τ1 becomes (Eq. 5.58): ε1 = F1 re,1 − fcr,1 + fsh,1 250.8 × 10−12 −618.4 × 10−15 = −618.4 × 10−15 5.658 × 10−15 −30 × 103 80.8 × 103 −1492 × 103 × − + 50 × 106 −70.3 × 106 −146.7 × 106 −385.7 × 10−6 = 0.841 × 10−6 mm−1 Therefore, εr,1 = −385.7 × 10−6 and κ1 = 0.841 × 10−6 mm−1 and the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε1(top) = εr,1 + (−200) × κ1 = −554.0 × 10−6 and ε1(btm) = εr,1 + 400 × κ1 = −49.0 × 10−6 The top and bottom ﬁbre concrete stresses at time τ1 are (Eq. 5.60): σc,1(top) = Ec,1 σc,1(btm) = Ec,1

" 1 y

# ε − ε 1 sh,1 + Fe,1,0 σc,0(top) = −2.21 MPa c,(top) & ' 1 yc,(btm) ε1 − εsh,1 + Fe,1,0 σc,0(btm) = 2.98 MPa

and the stresses in the reinforcement are: σs(1),1 = Es(1) 1 ys(1) ε1 = −102.4 MPa σs(2),1 = Es(2) 1 ys(2) ε1 = −18.2 MPa Based on these results the axial force and moment resisted by the concrete component at time τ1 are (Eq. 5.56):

Ac Bc εr1 rc,1 = Dc,1 ε1 + fcr,1 − fsh,1 = Ec,1 + fcr,1 − fsh,1 Bc Ic κ1 −385.7 × 10−6 177.6 × 103 17.46 × 106 = 28,000 × 0.841 × 10−6 17.46 × 106 6966 × 106 80.8 × 103 −1492 × 103 + − −70.3 × 106 −146.7 × 106 66.3 × 103 N = 51.9 × 106 Nmm

Uncracked sections 173

Time analysis – SSM (τ2 = 30,000 days) – time step 2 The cross-sectional rigidities at time τ2 are (Eqs 5.52): RA,2 = 5811 × 106 N; RB,2 = 631.3 × 109 Nmm; RI,2 = 255.8 × 1012 Nmm2 . and from Eqs 5.55b and 5.59:

5811 × 106 N 631.3 × 109 Nmm D2 = 631.3 × 109 Nmm 255.8 × 1012 Nmm2 −580.0 × 10−15 N−1 mm−1 235.1 × 10−12 N−1 F2 = −580.0 × 10−15 N−1 mm−1 5.339 × 10−15 N−1 mm−2 The creep effects due to the concrete stresses in the previous time steps, at τ0 and τ1 , and the shrinkage effects are obtained from Eqs 5.55c and d:

−44.9 × 103 fcr,2 = Fe,2,0 rc,0 + Fe,2,1 rc,1 = −0.986 × 39.1 × 106 66.3 × 103 −102.5 × 103 N − 2.214 × = −153.5 × 106 Nmm 51.9 × 106

Ac 177.6 × 103 fsh,2 = Ec,2 εsh,2 = × 30,000 × −600 × 10−6 6 Bc 17.46 × 10 −3196 × 103 N = −314.3 × 106 Nmm The strain distribution at time τ2 can be calculated as (Eq. 5.58): ε2 = F2 re,2 − fcr,2 + fsh,2 =

−670.1 × 10−6 1.220 × 10−6 mm−1

With εr,2 = −670.1 × 10−6 and κ2 = 1.220 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε2(top) = εr,2 + (−200) × κ2 = −914.2 × 10−6 ε2(btm) = εr,2 + 400 × κ2 = −181.9 × 10−6

174 Uncracked sections The top and bottom ﬁbre concrete stresses at τ2 are (Eq. 5.60): σc,2(top) = Ec,2

" # 1 yc,(top) ε2 − εsh,2 + Fe,2,0 σc,0(top) + Fe,2,1 σc,1(top)

= 30,000

! −670.1 × 10−6 −6 1 −200 − −600 × 10 1.220 × 10−6

− 0.986 × (−2.72) − 2.214 × (−2.21) = −1.85 MPa " # 1 yc,(btm) ε2 − εsh,2 + Fe,2,0 σc,0(btm) + Fe,2,1 σc,1(btm) σc,2(btm) = Ec,2 = 3.72 MPa The ﬁnal stresses in the reinforcement are: σs(1),2 = Es(1) 1 ys(1) ε2 = −170.6 MPa σs(2),2 = Es(2) 1 ys(2) ε2 = −48.6 MPa The stress and strain distributions at τ0 and at τ2 are shown in Fig. 5.13. Time, t0 Time, t2 −914.2

−108.9

−2.72

−1.85 −18.5

−170.6

x

−6

−1

k0 = 0.331 × 10 mm

σ

e

kk = 1.220 × 10−6mm−1

−48.6 y

(a) Cross-section

−181.9 89.8 (b) Strain diagram (× 10−6)

14.6

2.25 3.72 (c) Stress diagram (MPa)

Figure 5.13 Initial and ﬁnal strain and stress diagrams for Example 5.5.

Example 5.6 For the prestressed cross-section shown in Fig. 5.7 and analysed in Examples 5.2 and 5.4, determine the stress distribution at 30,000 days using the stepby-step procedure. The sustained external actions, Ne,j = −100 kN and Me,j = −50 kNm are applied at time τ0 = 28 days and kept constant with time. As for Example 5.5, the time domain is discretised into two time steps, from τ0 to τ1 and from τ1 to τ2 , with τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. The reinforcement is assumed to be linear-elastic and the relevant properties of

Uncracked sections 175 the concrete are: Ec,0 = 32 GPa; Ec,1 = 36 GPa; Ec,2 = 40 GPa; ϕ (τ0 , τ0 ) = 0; ϕ (τ1 , τ0 ) = 1.0; ϕ (τ2 , τ0 ) = 2.0; ϕ (τ1 , τ1 ) = 0; ϕ (τ2 , τ1 ) = 1.5; εsh (τ0 ) = εsh,0 = 0; εsh (τ1 ) = εsh,1 = −200 × 10−6 ; and εsh (τ2 ) = εsh,2 = −400 × 10−6 . The initial strains in the prestressing tendons prior to transfer is εp(1),init = εp(2),init = 0.00625 and the creep coefﬁcient for the prestressing steel is ϕp (τ1 , σp,init ) = 0.02 and ϕp (τ2 , σp,init ) = 0.03. The relevant creep functions for concrete are (Eqs 1.10 and 4.26a and b): J (τ0 , τ0 ) = 3.125 × 10−5 MPa−1 J (τ1 , τ1 ) = 2.777 × 10−5 MPa−1 J (τ2 , τ2 ) = 2.5 × 10−5 MPa−1 J (τ1 , τ0 ) = 6.25 × 10−5 MPa−1 J (τ2 , τ0 ) = 9.375 × 10−5 MPa−1 J (τ2 , τ1 ) = 6.944 × 10−5 MPa−1 Fe,1,0 = −1.25 Fe,2,0 = −0.972 Fe,2,1 = −1.777 Considering that the externally applied actions remain constant with time, for j = 0, 1 and 2: −100 × 103 N re,j = −50 × 106 Nmm

and 2000 × 103 N fp,init = 1290 × 106 Nmm

Short-term analysis (τ0 = 28 days) From Example 5.2: εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 . From Example 5.4: Ac = 312.7 × 103 mm2 ; Bc = 93.49 × 106 mm3 ; Ic = 76,960 × 106 mm4 . From Eq. 5.56, the stress resultants resisted by the concrete at τ0 are:

Ac Bc εr,0 0 0 rc,0 = Dc,0 ε0 + fcr,0 − fsh,0 = Ec,0 + − Bc Ic κ0 0 0 −1865 × 103 N = −1165 × 106 Nmm

176 Uncracked sections

Time analysis – SSM (τ1 = 100 days) – time step 1 From Eqs 5.52, the cross-sectional rigidities at time τ1 are: RA,1 = 12,120 × 106 N RB,1 = 3813 × 109 Nmm RI,1 = 3140 × 1012 Nmm2 and from Eq. 5.59:

133.6 × 10−12 N−1 mm−2 −162.2 × 10−15 N−1 mm−1 F1 = −162.2 × 10−15 N−1 mm−1 515.4 × 10−18 N−1

The effects of creep due to the concrete stresses calculated at τ0 and the effects of shrinkage are represented as: 2332 × 103 N −1865 × 103 fcr,1 = Fe,1,0 rc,0 = −1.25 × = 1456 × 106 Nmm −1165 × 106

Ac 312.7 × 103 −6 fsh,1 = Ec,1 εsh,1 = × 36,000 × −200 × 10 Bc 93.46 × 106 −2251 × 103 N = −673.2 × 106 Nmm

and the relaxation of the prestressing tendons is: fp.rel,1 =

Ap(1) Ep(1) εp(1),init

ϕp (τ1 , σp(1),init ) yp(1) Ap(1) Ep(1) εp(1),init Ap(2) Ep(2) εp(2),init + ϕp (τ1 , σp(2),init ) yp(2) Ap(2) Ep(2) εp(2),init

800 × 200,000 × 0.00625 = × 0.02 580 × 800 × 200,000 × 0.00625

800 × 200,000 × 0.00625 + × 0.02 710 × 800 × 200,000 × 0.00625 40 × 103 N = 25.8 × 106 Nmm

Uncracked sections 177 The strain distribution at time τ1 becomes: ε1 = F1 re,1 − fcr,1 + fsh,1 − fp,init + fp.rel,1 133.6 × 10−12 −162.2 × 10−15 = −162.2 × 10−15 515.4 × 10−18 −100 × 103 2332 × 103 −2251 × 103 × − + −50 × 106 1456 × 106 −673.2 × 106 2000 × 103 40 × 103 −328.8 × 10−6 − + = 1290 × 106 25.8 × 106 −0.697 × 10−6 mm−1 With εr,1 = −328.8 × 10−6 and κ1 = −0.697 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε1(top) = εr,1 + (−300) × κ1 = −119.6 × 10−6 and ε1(btm) = εr,1 + 850 × κ1 = −921.6 × 10−6 . The stresses in the top and bottom concrete ﬁbres at time τ1 are (Eqs 5.60): " # 1 yc,(top) ε1 − εsh,1 + Fe,1,0 σc,0(top) = 1.07 MPa σc,1(top) = Ec,1 & ' σc,1(btm) = Ec,1 1 yc,(btm) ε1 − εsh,1 + Fe,1,0 σc,0(btm) = −9.98 MPa and the stress in the non-prestressed reinforcement is:

3

−328.8 × 10−6 1 −240 −0.697 × 10−6

3

−328.8 × 10−6 1 790 −0.697 × 10−6

σs(1),1 = Es(1) 1 ys(1) ε1 = 200 × 10 = −32.3 MPa

σs(2),1 = Es(2) 1 ys(2) ε1 = 200 × 10 = −176.0 MPa

The stress in the prestressing steel is: σp(1),1 = Ep(1) 1 yp(1) ε1 + Ep(1) εp(1),init − εp.rel(1),1 −328.8 × 10−6 3 1 580 = 200 × 10 −0.697 × 10−6 + 200 × 103 × 0.00625 × (1 − 0.02) = 1078 MPa σp(2),1 = Ep(2) 1 yp(2) ε1 + Ep(2) εp(2),init − εp.rel(2),1 = 1060 MPa

178 Uncracked sections The axial force and moment resisted by the concrete component at time τ1 are (Eq. 5.56):

Ac Bc εr1 rc,1 = Dc,1 ε1 + fcr,1 − fsh,1 = Ec,1 + fcr,1 − fsh,1 Bc Ic κ1 −1465 × 103 N = −909.3 × 106 Nmm

Time analysis – SSM (τ2 = 30,000 days) – time step 2 The cross-sectional rigidities at time τ2 are (Eqs 5.52): RA,2 = 13,370 × 106 N RB,2 = 4187 × 109 Nmm RI,2 = 3448 × 1012 Nmm2 120.7 × 10−12 N−1 mm−2 −146.6 × 10−15 N−1 mm−1 F2 = −146.6 × 10−15 N−1 mm−1 468.1 × 10−18 N−1 Creep effects due to the concrete stresses in previous time steps, i.e. at τ0 and τ1 , are: fcr,2 = Fe,2,0 rc,0 + Fe,2,1 rc,1 −1465 × 103 −1865 × 103 = −0.972 × − 1.777 × −1165 × 106 −909.3 × 106 4418 × 103 N = 2749 × 106 Nmm and shrinkage effects are:

Ac 312.7 × 103 fsh,2 = Ec,2 εsh,2 = × 40,000 × −400 × 10−6 6 Bc 93.49 × 10 −5003 × 103 N = −1496 × 106 Nmm The relaxation of the prestressing tendons is: Ap(1) Ep(1) εp(1),init fp.rel,2 = ϕp (τ2 , σp(1),init ) yp(1) Ap(1) Ep(1) εp(1),init Ap(2) Ep(2) εp(2),init 60 × 103 N + ϕp (τ2 , σp(2),init ) = 38.7 × 106 Nmm yp(2) Ap(2) Ep(2) εp(2),init

Uncracked sections 179 The strain distribution at time τ2 is: ε2 = F2 re,2 − fcr,2 + fsh,2 − fp,init + fp.rel,2 =

−570.6 × 10−6 −0.915 × 10−6 mm−1

With εr,2 = −570.6 × 10−6 and κ2 = −0.915 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε2(top) = εr,2 + (−300) × κ2 = −295.8 × 10−6 and ε2(btm) = εr,2 + 850 × κ2 = −1349 × 10−6 The stresses in the top and bottom concrete ﬁbres at time τ1 are (Eqs 5.60): " # 1 yc,(top) ε2 − εsh,2 + Fe,2,0 σc,0(top) + Fe,2,1 σc,1(top) ! −570.6 × 10−6 −6 = 40,000 1 −300 − −400 × 10 −0.915 × 10−6

σc,2(top) = Ec,2

− 0.972 × 1.45 − 1.777 × 1.07 = 0.84 MPa " # 1 yc,(btm) ε2 − εsh,2 + Fe,2,0 σc,0(btm) + Fe,2,1 σc,1(btm) σc,2(btm) = Ec,2 = −7.77 MPa and the stresses in the non-prestressed reinforcement are:

3

−570.6 × 10−6 1 −240 −0.915 × 10−6

3

−570.6 × 10−6 1 790 −0.915 × 10−6

σs(1),2 = Es(1) 1 ys(1) ε2 = 200 × 10 = −70.1 MPa

σs(2),2 = Es(2) 1 ys(2) ε2 = 200 × 10 = −258.8 MPa

The ﬁnal stresses in the prestressing tendons are: σp(1),2 = Ep(1) 1 yp(1) ε2 + Ep(1) εp(1),init − εp.rel(1),2 = 992.1 MPa σp(2),2 = Ep(2) 1 yp(2) ε2 + Ep(2) εp(2),init − εp.rel(2),2 = 968.3 MPa

180 Uncracked sections The stress and strain distributions at τ0 and at τ2 are shown in Fig. 5.14. −295.8 45.5 −70.1

k2 = −0.915 × 10−6 mm−1

x

0.84 1.45 4.5

e

s

Time, t0 Time, t2

−6

k0 = −0.387 × 10 mm

−1349

y

−399.8

(b) Strain diagram (×

(a) Cross-section

−258.8

−1

−12.8

10−6)

−75.3

992.1 968.3

1191 1181

−7.77

(c) Stress diagram (MPa)

Figure 5.14 Initial and ﬁnal strain and stress diagrams for Example 5.6.

5.6 Composite steel-concrete cross-sections The analysis of composite steel-concrete cross-sections, such as those shown in Fig. 5.15, is presented here. Each cross-section has a single axis of symmetry and may be subjected to any combination of axial force and bending moment. In addition to the rolled or fabricated steel section or proﬁled decking, the concrete deck may contain layers of steel reinforcement. Mechanical shear connections are usually used to ensure that the steel-concrete interface is capable of carrying the imposed horizontal shear, and that the steel and concrete portions act compositely. For most practical steel-concrete composite sections, little slip occurs between the steel and the concrete under normal in-service conditions, with the magnitude of any slip depending on the rigidity of the interface connection (Refs 6–11). In the following, a perfect bond between the steel and the concrete is assumed.

..

.

.

.

.

.

.

.

.

. .

.

.

.

.

. . .

Steel reinforcement

Concrete . .. . . . . . . . . . . .. . . .. .. . . .. . . . . . . . . . . .. . . . . .. . . . . . . . . .

Steel

Concrete

Permanent steel formwork

Figure 5.15 Composite steel-concrete cross-sections.

Uncracked sections 181 The procedures for the short- and long-term analyses of the composite sections shown in Fig. 5.15 are similar to those presented for reinforced and prestressed concrete sections in Sections 5.3–5.5, except that the ﬂexural rigidity of the steel section (or its second moment of area) must be included, as well as its cross-sectional area. At any time instant τk , the internal axial force and moment resisted by the composite cross-section, Ni,k and Mi,k , respectively, may be expressed as: Ni,k = Nc,k + Ns,k + Nss,k

(5.63a)

Mi,k = Mc,k + Ms,k + Mss,k

(5.63b)

where Nc,k , Ns,k and Nss,k are the resultant axial forces in the concrete, the nonprestressed reinforcement and the steel part of the cross-section, respectively, and Mc,k , Ms,k and Mss,k are the corresponding moments about the reference axis. Since the rolled or fabricated steel (or permanent steel decking) does not creep or shrink, Nss,k and Mss,k may be deﬁned at any time τk as: Nss,k =

Ass

σss,k dA =

Ass

Mss,k =

Ass

Ess (εr,k + yκk ) dA = Ass Ess εr,k + Bs Ess κk

(5.64a)

yσss,k dA =

Ass

yEss (εr,k + yκk )d A = Bss Ess εr,k + Is Ess κk

(5.64b)

where Ass is the cross-sectional area of the rolled or fabricated steel section, and Bss and Iss are the ﬁrst and second moments of area of the steel section calculated with respect to the adopted reference axis. The constitutive relationship for the rolled or fabricated steel is assumed to be linear-elastic as follows: σss,k = Ess εk = Ess [1

y]εk

(5.65)

The advantage of this representation is that it describes both the instantaneous analysis (at τ0 ) and the time-dependent analysis (at τk ). At k = 0, Eqs 5.63 can be substituted into Eqs 5.2 to produce the governing equilibrium equations for a short-term analysis (as previously presented in Eq. 5.12). Using the AEMM for the time analysis (at τk ), Eqs 5.63 can be substituted into Eq. 5.24 to obtain the governing equations (previously presented in Eqs 5.34). The solution using the SSM is obtained by replacing Eqs 5.47 and 5.51 with Eqs 5.63 (and with time τj used instead of τk ). The only differences between the analyses of the composite steel-concrete crosssection and the analyses presented in Sections 5.3–5.5 are in the calculation of the cross-sectional rigidities, RA,k , RB,k and RI,k . The solution processes, involving the determination of the unknown strain and stress distributions at τk , are unchanged. For a composite steel-concrete cross-section, using the AEMM, the cross-sectional rigidities are: Ee,k + Ass Ess + RA,k = Ac

ms i=1

As(i) Es(i)

(5.66a)

182 Uncracked sections RB,j = Bc Ee,j + Bss Ess +

ms

ys(i) As(i) Es(i)

(5.66b)

i=1

Ee,j + Iss Ess + RI,j = Ic

ms

2 ys(i) As(i) Es(i)

(5.66c)

i=1

Ee,k = Ec,0 . When using the SSM, the concrete where for the short-term analysis at τ0 , modulus to be used in Eq. 5.66 is the one associated with the time step under consideration. As already discussed for reinforced and prestressed concrete sections, it is also common to transform the steel parts of the cross-section into equivalent areas of concrete, to calculate the rigidities of the transformed concrete section, and to use these in the analysis instead of the rigidities calculated using Eq. 5.66.

Example 5.7 The short-term and ﬁnal long-term behaviour of the composite cross-section shown in Fig. 5.16 is to be calculated. The cross-section is subjected to a sustained bending moment Me = 500 kNm. The axial force Ne in this example is zero. The time-dependent behaviour of the concrete is to be modelled using the AEMM and the relevant material properties are: Ec,0 = 25,000 MPa Ess = Es(1) = 200,000 MPa ϕ0∗ = ϕ (∞, τ0 ) = 2.5 χ0∗ = χ (∞, τ0 ) = 0.65 ∗ = εsh (∞) = −600 × 10−6 εsh

2400 75 75

150 dref = 450 x

600

y

As(1) = 2700 mm2 ys(1) = −375

Ass = 12,500 mm2 Iss = 750 μ 106 mm2 Centroid of Ass located at dref

Figure 5.16 Cross-sectional details for Example 5.7 (all dimensions in mm).

Uncracked sections 183 The external actions remain constant with time and are given by (with j = 0, k)

0N Ne,j = re,j = Me,j 500 × 106 Nmm

Short-term analysis (at time τ0 ) The geometric properties of the concrete slab are: Ac = bD−As(1) = 2400×150−2700 = 357,300 mm2 Bc = bD(D/2−dref )−As(1) ys(1) = 2400×150×(75−450)−2700×(−375) = −134.0×106 mm3

2 bD3 2400×1503 D 2 Ic = = +bD −dref −As(1) ys(1) 12 2 12 +2400×150×(75−450)2 −2700×(−375)2 = 50,920×106 mm4 The properties of the steel beam are already provided with respect to dref : Ass = 12,500 mm2 ; Bss = 0 mm3 (as the centroid of the steel beam is located on the reference axis); and Iss =750×106 mm4 . The cross-sectional rigidities are calculated using Eqs 5.66: RA,0 = Ac Ec,0 + Ass Ess +

ms

As(i) Es(i) = Ac Ec,0 + Ass Ess + As(1) Es(1)

i=1

= 11,970 × 106 N RB,0 = Bc Ec,0 + Bss Ess +

ms

ys(i) As(i) Es(i) = Bc Ec,0 + Bss Ess + ys(1) As(1) Es(1)

i=1 9

= −3552 × 10 Nmm RI,0 = Ic Ec,0 + Iss Ess +

ms

2 2 ys(i) As(i) Es(i) = Ic Ec,0 + Iss Ess + ys(1) As(1) Es(1)

i=1 12

= 1499 × 10 From Eq. 5.15: F0 = =

1

Nmm2

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 2.81 × 10−10 N−1

6.66 × 10−13 N−1 mm−1

6.66 × 10−13 N−1 mm−1 2.24 × 10−15 N−1 mm−2

184 Uncracked sections At time τ0 , before any creep or shrinkage has occurred, Eq. 5.14 reduces to: ε0 = F0 re,0 = =

2.81 × 10−10 6.66 × 10−13

6.66 × 10−13 2.24 × 10−15 333.3 × 10−6

0 500 × 106

1.123 × 10−6 mm−1

With εr,0 = 333.3 × 10−6 and κ0 = 1.123 × 10−6 mm−1 , the strains at the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε0(top) = εr,0 + (−450) × κ0 = −172.2 × 10−6 and ε0(btm) = εr,0 + 300 × κ0 = 670.4 × 10−6 The concrete stresses at the top and bottom of the slab at time τ0 are (Eq. 5.16a):

σc,0(top) = Ec,0 1 yc,(top)

333.3 × 10−6 ε0 = 25,000 1 −450 1.123 × 10−6

= −4.31 MPa σc,0(btm) = Ec,0

333.3 × 10−6 1 yc,(btm) ε0 = 25,000 1 −300 1.123 × 10−6

= −0.09 MPa The stress in the steel reinforcement is (Eq. 5.16b):

3

σs(1),0 = Es(1) 1 ys(1) ε0 = 200 × 10

333.3 × 10−6 1 −375 1.123 × 10−6

= −17.6 MPa The stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65): ! 333.3×10−6 & ' 3 1 −300 σss,0(top) = Ess 1 yss,(top) ε0 = 200×10 1.123×10−6 = −0.74 MPa

! " # −6 333.3×10 σss,0(btm) = Ess 1 yss,(btm) ε0 = 200×103 1 +300 1.123×10−6 = 134 MPa

Uncracked sections 185 The stress resultants resisted by the concrete at τ0 can be determined from:

Nc,0 Ac Bc εr,0 −785.8 × 103 N rc,0 = = = Dc,0 ε0 = Ec,0 313.6 × 106 Nmm Bc Ic κ0 Mc,0

Time analysis – AEMM (at time τk = ∞) From Eqs 4.35 and 4.46: Ee,k =

25,000 = 9524 MPa 1 + 0.65 × 2.5

2.5 × (0.65 − 1.0) Fe,0 = = −0.333 1.0 + 0.65 × 2.5 The cross-sectional rigidities at time τk are (Eq. 5.66): RA,k = Ac Ee,k + Ass Ess + As(1) Es(1) = 6443 × 106 N Ee,k + Bss Ess + ys(1) As(1) Es(1) = −1479 × 109 Nmm RB,k = Bc 2 Ee,k + Iss Ess + ys(1) As(1) Es(1) = 710.9 × 1012 Nmm2 RI,k = Ic

Fk is then obtained using Eq. 5.40: Fk =

1

RI,k −RB,k −RB,k RA,k

RA,k RI,k − R2B,k 2.96 × 10−10 N−1 6.17 × 10−13 N−1 mm−1 = 6.17 × 10−13 N−1 mm−1 2.69 × 10−15 N−1 mm−2

The creep effects at τk due to the concrete stresses calculated at τ0 are calculated using Eq. 5.36: 3 3 N 261.9 × 10 −785.8 × 10 fcr,k = = Fe,0 rc,0 = −0.333 × −104.6 × 106 Nmm 313.6 × 106

and the shrinkage effects are given by Eq. 5.37:

357,300 × 9524 Ac fsh,k = −600 × 10−6 Ee,k εsh,k = 6 Bc −134 × 10 × 9524 −2042 × 103 N = 765.6 × 106 Nmm

186 Uncracked sections From Eq. 5.39, the ﬁnal strain distribution at time τk is: εk = Fk re,k − fcr,k + fsh,k =

162.2 × 10−6

2.265 × 10−6 mm−1

With εr,k = 162.2 × 10−6 and κk = 2.265 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): εk(top) = εr,k + (−450) × κk = −856.9 × 10−6 εk(btm) = εr,k + 300 × κk = 841.6 × 10−6 The ﬁnal concrete stresses at the top and bottom of the slab at time τk are (Eq. 5.41a): & ' 1 yc,(top) εk − εsh,k + Fe,0 σc,0 ! 162.2 × 10−6 −6 − −600 × 10 = 9524 1 −450 2.265 × 10−6

σc,k(top) = Ee,k

− 0.333 × (−4.31) = −1.01 MPa " # 1 yc,(btm) εk − εsh,k + σc,k(btm) = Ee,k Fe,0 σc,0 = 0.82 MPa The ﬁnal stress in the steel reinforcement is (Eq. 5.41b):

3

σs(1),k = Es(1) 1 ys(1) εk = 200 × 10

162.2 × 10−6 1 −375 2.265 × 10−6

= −137.4 MPa and the ﬁnal stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65):

3

σss,k(top) = Ess 1 yss,(top) εk = 200 × 10

162.2 × 10−6 1 −300 2.265 × 10−6

= −103.4 MPa

σss,k(btm) = Ess 1 yss,(btm) εk = 200 × 103 = 168.3 MPa

162.2 × 10−6 1 300 2.265 × 10−6

Uncracked sections 187 The ﬁnal stress and strain distributions are illustrated in Fig. 5.17. −856.9

−172.2

−4.31 −1.01

−17.6

−137 −103

kk = 2.265 × 10−6 mm−1 e

x Time, t0 −6 −1 Time, tk k0 = 1.123 × 10 mm

−0.74 Steel stress

670.4 841.6

y (a) Cross-section

−6)

(b) Strain diagram (×10

−0.09 0.82 Concrete stress

s

134 168 (c) Stress diagram (MPa)

Figure 5.17 Stress and strain distributions due to Me = 500 kNm (Example 5.7).

As can be seen in Fig. 5.17, the effect of creep and shrinkage in the concrete portions of a composite section in positive bending is to substantially increase positive curvature with time. In this example, the initial curvature has approximately doubled (from κ0 = 1.123 × 10−6 mm−1 to κk = 2.265 × 10−6 mm−1 ). In addition, the concrete deck has been relieved of much of its initial compression, with tensile stress developing in the bottom concrete ﬁbres. The steel I-section therefore carries signiﬁcantly more of the external moment after a period of sustained loading. Both the tensile stresses in the bottom ﬁbres of the steel I-section and the compressive stresses in the top ﬁbres have increased substantially with time.

Example 5.8 In order to examine the effects of shrinkage on the behaviour of a composite section, the cross-section shown in Fig. 5.16 (and analysed in Example 5.7) is here re-analysed for the case when Me = 0 and Ne = 0. As in Example 5.7, the ﬁnal shrinkage is −600 × 10−6 . This unloaded situation is quite common in practice, for example near the supports of a simply-supported member or at the points of contraﬂexure in a continuous composite girder. Obviously, in the short-term, the section is unloaded, with zero deformation (εr,0 = 0 and κ0 = 0) and no external actions. As time increases, the concrete deck shrinks while being restrained by the steel I-section and by the bonded steel reinforcement. As for Example 5.7: Ee,k = 9524 MPa; Fe,0 = −0.333; Ac = 2 6 3 357,300 mm ; Bc = −134 × 10 mm ; Ic = 50,920 × 106 mm4 ; RA,k = 6443 × 106 N; RB,k = −1479 × 109 Nmm; RI,k = 710.9 × 1012 Nmm2 ; and Fk =

2.96 × 10−10 N−1

6.17 × 10−13 N−1 mm−1

6.17 × 10−13 N−1 mm−1 2.69 × 10−15 N−1 mm−2

188 Uncracked sections With no external loads and from Eqs 5.36 and 5.37:

0N re,0 = re,k = 0 Nmm

0N fcr,k = 0 Nmm −2042 × 103 N fsh,k = 765.6 × 106 Nmm The ﬁnal strain distribution at time τk becomes (Eq. 5.39): εk = Fk re,k − fcr,k + fsh,k =

−133.4 × 10−6 N

+0.799 × 10−6 Nmm

With εr,k = −133.4 × 10−6 and κk = +0.799 × 10−6 mm−1 , the ﬁnal strain at the top of the slab (y = −450 mm) and at the bottom of the steel I-section (y = 300 mm) at time τk are: εk(top) = εr,k + (−450) × κk = −493.2 × 10−6 εk(btm) = εr,k + 300 × κk = +106.5 × 10−6 The ﬁnal concrete stresses at the top and bottom of the slab at time τk are (Eq. 5.41a): σc,k(top) = 9524

! −133.4 × 10−6 1 −450 − (−600 × 10−6 ) 0.799 × 10−6

= +1.02 MPa

! −133.4 × 10−6 −6 σc,k(btm) = 9524 1 −300 − (−600 × 10 ) 0.799 × 10−6 = +2.16 MPa and the ﬁnal stress in the steel reinforcement is (Eq. 5.41b): σs(1),k = 200,000 [−133.4 − 375 × 0.799] × 10−6 = −86.6 MPa The ﬁnal stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65): σss,k(top) = 200,000 [−133.4 − 300 × 0.799] × 10−6 = −74.6 MPa σss,k(btm) = 200,000 [−133.4 + 300 × 0.799] × 10−6 = +21.3 MPa

Uncracked sections 189 The ﬁnal stress and strain distributions are illustrated in Fig 5.18. The shrinkageinduced ﬁnal curvature (+0.799 × 10−6 mm−1 ) is almost 70 per cent of the change in curvature with time in Example 5.7 (where κ = κk − κ0 = 1.142 × 10−6 mm−1 ). In addition, the tensile stress induced in the bottom ﬁbre of the concrete due to the restraint to shrinkage may be sufﬁcient to cause cracking in the concrete. −493.2

1.02

−86.6

2.16

−74.6 e

x

y (a) Cross-section

s

106.5 (b) Strain diagram (× 10−6)

21.3 (c) Stress diagram (MPa)

Figure 5.18 Shrinkage-induced stress and strain distributions at τk for Example 5.8.

5.7 Composite concrete-concrete cross-sections The analysis of a cross-section consisting of different reinforced or prestressed concrete elements acting compositely together and subjected to a sustained bending moment and axial force is presented here. A typical cross-section is shown in Fig 5.19. This particular cross-section is made up of two concrete elements, a precast pretensioned I-section (Element 1) and an in-situ slab deck (Element 2). Each concrete element may have different creep and shrinkage characteristics, as well as different elastic moduli. In the subsequent analyses, perfect bond is assumed between each concrete element, as well as between the concrete and the bonded steel reinforcement.

ds(1) As(1) ds(3) ds(2)

As(3)

dref ds(4)

dp(2)

dc(2)

As(2)

dp(1)

x

Centroidal axis of precast concrete girder (Element 1), Ac(1)

dc(1)

Centroidal axis of in-situ concrete deck (Element 2), Ac(2)

Ap(1) Ap(2) As(4) y

Figure 5.19 Typical concrete-concrete composite section.

190 Uncracked sections The general procedure introduced in Sections 5.3–5.5 for reinforced and prestressed concrete cross-sections is readily extended to include composite sections comprising two or more concrete components. Consider a composite section formed with mc different concrete components. For the i-th concrete component (with i = 1, . . . , mc ), the area is Ac(i) , and the ﬁrst and second moments of the area about the reference axis are Bc(i) and Ic(i) , respectively. For clarity and completeness, the short-term analysis (assuming linear-elastic material behaviour) and the time-dependent analyses using both the AEMM and the SSM are presented separately in the following. 5.7.1 Short-term analysis As outlined in Section 5.3, the constitutive relationships for each material for use in the instantaneous analysis are (Eq. 5.4): σc(i),0 = Ec(i),0 ε0

(5.67a)

σs(i),0 = Es(i) ε0 σp(i),0 = Ep(i) ε0 + εp(i),init

(5.67b) (5.67c)

Similar to Eq. 5.7a, the internal actions carried by the i-th concrete element (for inclusion in the equilibrium equations) can be expressed as: Nc(i),0 =

Ac(i)

σc(i),0 dA =

Ac(i)

Ec(i),0 εr,0 + yκ0 dA

= Ac(i) Ec(i),0 εr,0 + Bc(i) Ec(i),0 κ0 Mc(i),0 = yσc(i),0 dA = Ec(i),0 y εr,0 + yκ0 dA Ac(i)

(5.68a)

Ac(i)

= Bc(i) Ec(i),0 εr,0 + Ic(i) Ec(i),0 κ0

(5.68b)

and, as in Eq. 5.12, the governing system of equilibrium equations is: re,0 = D0 ε0 + fp,init

(5.69)

Solving for the unknown strain variables gives (Eq. 5.14): ε0 = D−1 re,0 − fp,init = F0 re,0 − fp,init 0

(5.70)

where D0 = F0 =

RA,0 RB,0 RB,0 RI,0 1 RA,0 RI,0 − R2B0

(5.71a)

RI,0 −RB,0 −RB,0 RA,0

(5.71b)

Uncracked sections 191

εr,0 ε0 = κ0

Ne,0 re,0 = Me,0 mp Ap(i) Ep(i) εp(i),init fp,init = yp(i) Ap(i) Ep(i) εp(i),init i=1

(5.71c) (5.71d)

(5.71e)

The cross-sectional rigidities forming the D0 matrix in Eq. 5.71a are: RA,0 =

mc

Ac(i) Ec(i),0 +

ms

i=1

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ec(i),0 + RA,s + RA,p

i=1

(5.72a) RB,0 =

mc

Bc(i) Ec(i),0 +

i=1

=

ms

ys(i) As(i) Es(i) +

i=1

mc

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ec(i),0 + RB,s + RB,p

(5.72b)

i=1

RI,0 =

mc

Ic(i) Ec(i),0 +

i=1

=

ms

2 ys(i) As(i) Es(i) +

i=1

mc

Ic(i) Ec(i),0 + RI,s + RI,p

mp

2 yp(i) Ap(i) Ep(i)

i=1

(5.72c)

i=1

where for convenience the following notation is introduced for the rigidities of the reinforcement and tendons: ms As(i) Es(i) (5.73a) RA,s = i=1

RB,s =

ms

ys(i) As(i) Es(i)

(5.73b)

2 ys(i) As(i) Es(i)

(5.73c)

i=1

RI,s =

ms i=1 mp

RA,p =

Ap(i) Ep(i)

(5.74a)

yp(i) Ap(i) Ep(i)

(5.74b)

2 yp(i) As(i) Ep(i)

(5.74c)

i=1

RB,p =

mp i=1

RI,p =

mp i=1

192 Uncracked sections The stress distribution is calculated from Eq. 5.16: σc(i),0 = Ec(i),0 ε0 = Ec(i),0 [1

y]ε0

σs(i),0 = Es(i) ε0 = Es(i) [1 ys(i) ]ε0 σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) [1

(5.75a) (5.75b) yp(i) ]ε0 + Ep(i) εp(i),init

(5.75c)

where ε0 = εr,0 + yκ0 = [1 y]ε0 . 5.7.2 Time analysis – AEMM For the analysis of stresses and deformations on a composite concrete-concrete crosssection at time τk after a period of sustained loading, the AEMM may be used, as outlined in Section 5.4. The stress–strain relationships for each concrete element and for each layer of reinforcement and tendons at τk are as follows (Eq. 5.22): σc(i),k = Fe(i),0 σc(i),0 Ee(i),k εk − εsh(i),k + σs(i),k = Es(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(5.76a) (5.76b) (5.76c)

In this case the contribution of the i-th concrete component to the internal axial force and moment can be determined as (similar to Eq. 5.27): Nc(i),k =

Ac(i)

σc(i),k dA =

Ac(i)

Ee(i),k εr,k + yκk − εsh(i),k + Fe(i),0 σc(i),0 dA

= Ac(i) Ee(i),k εr,k + Bc(i) Ee(i),k κk − Ac(i) Ee(i),k εsh(i),k + Fe(i),0 Nc(i),0 (5.77a) Mc(i),k = yσc(i),k dA = y Ee(i),k εr,k + yκk − εsh(i),k + Fe(i),0 σc(i),0 dA Ac(i)

Ac(i)

= Bc(i) Ee(i),k εr,k + Ic(i) Ee(i),k κk − Bc(i) Ee(i),k εsh(i),k + Fe(i),0 Mc(i),0

(5.77b)

The equilibrium equations are (Eq. 5.34): re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k

(5.78)

and solving gives the strain at time τk (Eq. 5.39): εk = D−1 re,k − fcr,k + fsh,k − fp,init + fp.rel,k k = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(5.79)

Uncracked sections 193 where

ε εk = r,k κk

Ne,k re,k = Me,k

RA,k RB,k Dk = RB,k RI,k Fk =

1

(5.80a) (5.80b) (5.80c)

RI,k

−RB,k

RA,k RI,k − R2B,k −RB,k

(5.80d)

RA,k

and the cross-sectional rigidities at τk are:

RA,k =

mc

Ac(i) Ee(i),k +

i=1

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ee(i),k + RA,s + RA,p

i=1

(5.81a) RB,k =

mc

Bc(i) Ee(i),k +

i=1

=

mc

ms

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ee(i),k + RB,s + RB,p

(5.81b)

i=1

RI,k =

mc

Ee(i),k + Ic(i)

i=1

=

mc

ms

2 ys(i) As(i) Es(i) +

mp

2 yp(i) Ap(i) Ep(i)

i=1

i=1

Ee(i),k + RI,s + RI,p Ic(i)

(5.81c)

i=1

In Eq. 5.78, the effects of creep and shrinkage of the concrete elements are included by (see Eqs 5.36 and 5.37):

fcr,k =

mc

Fe(i),0

i=1

fsh,k =

mc Ac(i) i=1

Bc(i)

Nc(i),0 Mc(i),0

=

mc i=1

Ee(i),k εsh(i),k

Fe(i),0 Ec(i),0

Ac(i) εr,0 + Bc(i) κ0 Bc(i) εr,0 + Ic(i) κ0

(5.82)

(5.83)

194 Uncracked sections The initial strain in the prestressing steel and relaxation are accounted for using (Eq. 5.38): fp,init =

mp i=1

fp.rel,k =

mp

Ap(i) Ep(i) εp(i),init

yp(i) Ap(i) Ep(i) εp(i),init

i=1

Ap(i) Ep(i) εp(i),init ϕp (τk , σp(i),init ) yp(i) Ap(i) Ep(i) εp(i),init ϕp (τk , σp(i),init )

(5.84a)

(5.84b)

The stress distributions at time τk in each concrete element and in the reinforcement and tendons are (Eq. 5.41): Fe(i),0 σc(i),0 Ee(i),k εk − εsh(i),k + σc(i),k = & ' = Ee(i),k 1 y εk − εsh(i),k + Fe(i),0 σc(i),0 σs(i),k = Es(i) εk = Es(i) 1 ys(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(5.85a) (5.85b)

(5.85c)

where εk = εr,k + yκk = 1 y εk .

Example 5.9 The composite cross-section shown in Fig. 5.20 forms part of a bridge deck and consists of an in-situ reinforced concrete deck and a precast post-tensioned I-section (with bonded tendons). At time τ0 with both concrete elements acting compositely, the road surface and other superimposed dead load are placed on the bridge, thereby introducing an increment of external moment Me = 400 kNm at the section shown. Both the immediate and ﬁnal long-term changes of stress caused by Me are to be calculated. For the precast I-girder: Ec(1) (τ0 ) = 32,000 MPa; ϕ(1) (∞, τ0 ) = 2.0; χ(1) (∞, τ0 ) = 0.65. For the concrete deck: Ec(2) (τ0 ) = 25,000 MPa; ϕ(2) (∞, τ0 ) = 2.5; χ(2) (∞, τ0 ) = 0.65. For the steel reinforcement and tendons: Es = Ep = 200,000 MPa. In this example, only the increments of stress and strain caused by Me are to be calculated. In the actual bridge girder, these must be added to the increments of stress and strain caused by the prestress, self-weight, live load, shrinkage of the concrete, relaxation of the prestressing steel and, if applicable, temperature changes.

Uncracked sections 195 As(1) = 2700 mm2 2400

75 210 1030 1160 1240

x 150

As(2) = 900 mm2 752 Centroidal axis of precast concrete I-girder Ac(1) = 317 × 103 mm2 Ic(1) = 49,900 × 106 mm4

Centroidal axis of in-situ concrete slab

1300

Ap(1) = 800 mm2 Ap(2) = 800 mm2 As(3) = 1800 mm2 y

Figure 5.20 Details of the cross-section for Example 5.9.

In the following solution, the top surface of the in-situ slab is selected as the reference axis, as shown in Fig. 5.20, (i.e. dref = 0 mm) and its distances from the steel layers are: ys(1) = 75 mm, ys(2) = 210 mm, ys(3) = 1240 mm, yp(1) = 1030 mm and yp(2) = 1160 mm. The applied loads are:

0N re,0 = 400 × 106 Nmm As no prestressing forces and shrinkage effects are considered in this problem, the vectors f p,init , f p.rel,0 , f p.rel,k and f sh,k are all nil:

0N fp,init = 0 Nmm

0N fp.rel,0 = fp.rel,k = 0 Nmm

0N fsh,k = 0 Nmm

Short-term analysis (at time τ0 ) The geometric properties of the precast girder cross-section are calculated as: Ac(1) = Agross − As(2) − As(3) − Ap(1) − Ap(2) = 312,700 mm2 Bc(1) = Agross dc(1) − dref − As(2) ys(2) + As(3) ys(3) − Ap(1) yp(1) + Ap(2) yp(2) = 234.2 × 106 mm3 2 2 2 Ic(1) = Igross + Agross dc(1) − dref − As(2) ys(2) + As(3) ys(3) 2 2 − Ap(1) yp(1) + Ap(2) yp(2) = 224.4 × 109 mm4

196 Uncracked sections and those of the concrete deck are: Ac(2) = bD − As(1) = 357,300 mm2 Bc(2) = bD(D/2 − dref ) − As(1) ys(1) = 26.79 × 106 mm3

2 bD3 D 2 Ic(2) = + bD − dref − As(1) ys(1) = 2684 × 106 mm4 12 2 The instantaneous cross-sectional rigidities are (Eq. 5.72): RA,0 = Ac(1) Ec(1),0 + Ac(2) Ec(2),0 + As(1) + As(2) + As(3) Es + Ap(1) + Ap(2) Ep = 20,340 × 106 N RB,0 = Bc(1) Ec(1),0 + Bc(2) Ec(2),0 + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 9039 × 109 Nmm 2 2 2 RI,0 = Ic(1) Ec(1),0 + Ic(2) Ec(2),0 + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 8198 × 1012 Nmm2 The matrix F0 can then be determined as (Eq. 5.71b): F0 =

1

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 −106.3 × 10−15 N−1 mm−1 96.42 × 10−12 N−1 = −106.3 × 10−15 N−1 mm−1 239.2 × 10−18 N−1 mm−2

The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.70:

96.42 × 10−12 −106.3 × 10−15 −106.3 × 10−15 239.2 × 10−18 ( ) 0 0 −42.5 × 10−6 × − = 0 400 × 106 0.095 × 10−6 mm−1

ε0 = F0 re,0 − fp,init =

The increment of strain at the reference axis and the increment of curvature caused by the imposed moment Me = 400 kNm are therefore εr,0 = −42.5×10−6 and κ0 = 0.095×10−6 mm−1 and, from Eq. 5.1, the increments of top (y = 0 mm) and bottom (y = 1300 mm) ﬁbre strains are: ε0(top) = εr,0 + 0 × κ0 = −42.5 × 10−6 and ε0(btm) = εr,0 + 1300 × κ = 81.8 × 10−6

Uncracked sections 197 From Eq. 5.75a, the changes in the top and bottom ﬁbre stresses on the precast I-section are: σc(1),0(top) = Ec(1),0 εc(1),0(top) = 32,000 × (−42.5 + 150 × 0.095) × 10−6 = −0.90 MPa σc(1),0(btm) = Ec(1),0 εc(1),0(btm) = 32,000 × (−42.5 + 1300 × 0.095) × 10−6 = +2.62 MPa and on the concrete deck: σc(2),0(top) = Ec(2),0 εc(2),0(top) = 25,000 × (−42.5 + 0 × 0.095) × 10−6 = −1.06 MPa σc(2),0(btm) = Ec(2),0 εc(2),0(btm) = 25,000 × (−42.5 + 150 × 0.095) × 10−6 = −0.70 MPa The increments of stress in the non-prestressed reinforcement are obtained from Eq. 5.75b as: −42.5 × 10−6 3 σs(1),0 = 200 × 10 × 1 75 = −7.1 MPa 0.095 × 10−6 −6 −42.5 × 10 σs(2),0 = 200 × 103 × 1 210 = −4.5 MPa 0.095 × 10−6 −42.5 × 10−6 3 σs(3),0 = 200 × 10 1 1240 = 15.2 MPa 0.095 × 10−6 and in the prestressing steel (Eq. 5.75c)

σp(1),0 = Ep 1 yp(1)

−42.5 × 10−6 ε0 = 200 × 10 × 1 1030 0.095 × 10−6

−42.5 × 10−6 ε0 = 200 × 10 × 1 1160 0.095 × 10−6

= 11.2 MPa

σp(2),0 = Ep 1 yp(2)

3

3

= 13.7 MPa

Long-term analysis (at time τk = ∞) For the long-term analysis at time τk the age-adjusted material properties for the two concrete elements are obtained from Eqs 4.35 and 4.46: Ee(1),k =

Ec(1),0 32,000 = 13,910 MPa = 1 + χ(1) (τk , τ0 ) ϕ(1) (τk , τ0 ) 1 + 0.65 × 2.0

198 Uncracked sections Ec(2),0 25,000 = 9523 MPa = 1 + χ(2) (τk , τ0 ) ϕ(2) (τk , τ0 ) 1 + 0.65 × 2.5 ϕ(1) (τk , τ0 ) χ(1) (τk , τ0 ) − 1 2.0 × (0.65 − 1) Fe(1),0 = = −0.304 = 1 + χ(1) (τk , τ0 ) ϕ(1) (τk , τ0 ) 1 + 0.65 × 2.0 ϕ(2) (τk , τ0 ) χ(2) (τk , τ0 ) − 1 2.5 × (0.65 − 1) Fe(2),0 = = −0.333 = 1 + 0.65 × 2.5 1 + χ(2) (τk , τ0 ) ϕ(2) (τk , τ0 ) Ee(2),k =

Creep effects are accounted for using Eq. 5.82:

Ac(1) εr,0 + Bc(1) κ0 Ac(2) εr,0 + Bc(2) κ0 fcr,k = Fe(1),0 Ec(1),0 + Fe(2),0 Ec(2),0 Bc(1) εr,0 + Ic(1) κ0 Bc(2) εr,0 + Ic(2) κ0 16.5 × 103 N = −104.8 × 106 Nmm The cross-sectional rigidities at time τk are calculated from Eq. 5.81: RA,k = Ac(1) Ee(1),k + Ac(2) Ee(2),k + As(1) + As(2) + As(3) Es + Ap(1) + Ap(2) Ep = 9153 × 106 N RB,k = Bc(1) Ee(1),k + Bc(2) Ee(2),k + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 4389 × 109 Nmm 2 2 2 RI,k = Ic(1) Ee(1),k + Ic(2) Ee(2),k + As(1) ys(1) Es + As(2) ys(2) + As(3) ys(3) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 4097 × 1012 Nmm2 Matrix Fk is then determined as (Eq. 5.80d): −240.5 × 10−15 N−1 mm−1 224.6 × 10−12 N−1 Fk = −240.5 × 10−15 N−1 mm−1 501.7 × 10−18 N−1 mm−2 The strain vector εk at time τk caused by the sustained moment Me is obtained from Eq. 5.79: −125.1 × 10−6 N εk = Fk re,k − fcr,k = 0.257 × 10−6 Nmm The ﬁnal increments of strains at the top and bottom ﬁbres of the cross-section are (Eq. 5.1): εk(top) = εr,k + 0 × κk = −125.1 × 10−6 εk(btm) = εr,k + 1300 × κk = 209.2 × 10−6

Uncracked sections 199 The increments of stress at time τk in the top and bottom ﬁbres of the precast I-section are determined using Eq. 5.85a: σc(1),k(top) = Fe(1),0 σc(1),0(top) Ee(1),k εc(1),k(top) − εsh(1),k + = 13,913 × (−125.1 + 150 × 0.257) × 10−6 − 0.304 × (−0.90) = −0.93 MPa and Ee(1),k εc(1),k(btm) − εsh(1),k + Fe(1),0 σc(1),0(btm) = 2.11 MPa σc(1),k(btm) = Similarly, for the concrete deck: σc(2),k(top) = Ee(2),k εc(2),k(top) − εsh(2),k + Fe(2),0 σc(2),0(top) = 9523 × (−125.1 + 0 × 0.257) × 10−6 − 0.333 × (−1.06) = −0.84 MPa Fe(2),0 σc(2),0(btm) = −0.59 MPa Ee(2),k εc(2),k(btm) − εsh(2),k + σc(2),k(btm) = The ﬁnal increments of stress in the non-prestressed reinforcement are obtained from Eq. 5.85b: −125.1 × 10−6 σs(1),k = 200 × 10 × 1 75 = −21.2 MPa 0.257 × 10−6 −125.1 × 10−6 3 σs(2),k = 200 × 10 × 1 210 = −14.2 MPa 0.257 × 10−6 −125.1 × 10−6 3 σs(3),k = 200 × 10 1 1240 = +38.8 MPa 0.257 × 10−6 3

and for the prestressing steel, Eq. 5.85c gives: σp(1),k = Ep 1 yp(1) εk + Ep εpinit(1) −6 −125.1 × 10 + 0 = 27.9 MPa = 200 × 103 × 1 1030 0.257 × 10−6 and σp(2),k = Ep 1 yp(2) εk + Ep εpinit(2) −6 −125.1 × 10 = 200 × 103 × 1 1160 + 0 = 34.6 MPa 0.257 × 10−6

200 Uncracked sections The stress and strain distributions at times τ0 and at τk are shown in Fig. 5.21.

x

−125.1 −42.5

−1.06 −0.84 s −7.1 −21.2 −0.93−0.90 −4.5 −0.70 −0.59 −14.2

e

Time, t0 Time, tk 11.2 13.7 15.2

y (a) Cross-section

81.8 209.2 (b) Strain diagram (× 10−6)

27.9 34.6 38.8 2.11 2.62 (c) Stress diagram (MPa)

Figure 5.21 Strain and stress distributions for Example 5.9.

5.7.3 Time analysis – SSM The SSM outlined in Section 5.5 is extended in the following to analyse a composite cross-section with mc different concrete elements. Similar to Eqs 4.25 and 5.44, the constitutive relationships for the different materials at time τj are: j−1

σc(i),j = Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n

(5.86a)

n=0

σs(i),j = Es(i) εj − εs(i),set−1 σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j − εp(i),set−1

(5.86b) (5.86c)

where the additional strain terms εc(i),set−1 , εs(i),set−1 , εp(i),set−1 have been included to account for variations in the cross-section when different parts of the cross-section are cast at different times, such as occurs, for example, in sequential casting. The term set refers to the time step at which a particular concrete element sets and begins to contribute to the structural stiffness. The inclusion of the strains εc(i),set−1 , εs(i),set−1 , εp(i),set−1 in Eq. 5.86 ensures that all new components are initially unloaded. Similar treatment can be given to the grouting of post-tensioning ducts at some time after the transfer of prestress, as illustrated subsequently in Example 5.10. In the formulation adopted here (and illustrated in Example 5.10), two steps are considered in the solution whenever a new concrete element is added to the crosssection. The ﬁrst step involves the calculation of the cross-sectional response just before the element sets, at τset−1 , and the second step involves the calculation of the response just after the element starts to contribute to the structural stiffness, at τset . Obviously, for situations not related to sequential casting, i.e. where all concrete elements are in place from the beginning of the analysis, the terms εc(i),set−1 , εs(i),set−1 and εp(i),set−1 in Eq. 5.86 are all set to zero.

Uncracked sections 201 Similarly to Eq. 5.48, the axial force and moment resisted by the i-th concrete element are: ⎡ ⎤ j−1 ⎣Ec(i),j εj − εsh(i),j − εc(i),set−1 + Nc(i),j = σc(i),j dA = Fe(i),j,n σc(i),n⎦ dA Ac(i)

Ac(i)

n=0

= Ac(i) Ec(i),j εr,j − εr,set−1 + Bc(i) Ec(i),j κj − κset−1 − Ac(i) Ec(i),j εsh(i),j +

j−1

Fe(i),j,n Nc(i),n

n=0

Mc(i),j =

yσc(i),j dA =

Ac(i)

(5.87a) ⎡

⎤ j−1 y ⎣Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n⎦ dA

Ac(i)

n=0

= Bc(i) Ec(i),j εr,j − εr,set−1 + Ic(i) Ec(i),j κj − κset−1 − Bc(i) Ec(i),j εsh(i),j +

j−1

Fe(i),j,n Mc(i),n

(5.87b)

n=0

in which εr,set−1 and κset−1 deﬁne the strain diagram immediately before the i-th concrete element sets at τset−1 . As for the earlier analyses (Eq. 5.54), the governing equilibrium equations are: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j − fset,j

(5.88)

and solving for the unknown strain distribution at τj gives: re,j − fcr,j + fsh,j − fp,init + fp.rel,j + fset,j εj = D−1 j = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j + fset,j

(5.89)

where (as before):

εr,j κj

RA,j RB,j Dj = RB,j RI,j

Ne,j re,j = Me,j εj =

Fj =

fp,init =

1

(5.90a) (5.90b) (5.90c)

RI,j −RB,j −RB,j RA,j

RA,j RI,j − R2B,j mp Ap(i) Ep(i) εp(i),init i=1

yp(i) Ap(i) Ep(i) εp(i),init

(5.90d)

(5.90e)

202 Uncracked sections mp Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) fp.rel,j = yp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) i=1 fcr,j =

j−1 mc

(5.90f)

Fe(i),j,n rc(i),n

(5.90g)

i=1 n=0

fsh,j =

mc Ac(i) i=1

Bc(i)

Ec(i),j εsh(i),j

(5.90h)

while f set.j is deﬁned as:

fset,j =

mc

fc(i).set,j +

i=1

ms

fs(i).set,j +

i=1

mp

fp(i).set,j

(5.90i)

i=1

and fc(i).set,j = fs(i).set,j =

Ac(i) Ec(i),j εr,set−1 + Bc(i) Ec(i),j κset−1

(5.90j)

Bc(i) Ec(i),j εr,set−1 + Ic(i) Ec(i),j κset−1 As(i) Es(i) εr,set−1 + Bs(i) Es(i) κset−1

fp(i).set,j =

Bs(i) Es(i) εr,set−1 + Is(i) Es(i) κset−1 Ap(i) Ep(i) εr,set−1 + Bp(i) Ep(i) κset−1

(5.90k)

(5.90l)

Bp(i) Ep(i) εr,set−1 + Ip(i) Ep(i) κset−1

The i-th component of the cross-section is included in the calculation of f set,j only when the instant in time τj is greater than or equal to τset of the i-th component. The axial force and moment resisted by the concrete at any time τi (required in Eq. 5.90g) is determined as: rc(i),n =

Nc(i),n

Mc(i),n

= Dc(i),n (εn − εset−1 ) +

n−1

Fe(i),n,l rc(i),l −

l=0

Ac(i) Bc(i)

Ec(i),n εsh(i),n (5.91)

where εset−1 is the vector containing εr,set−1 and κset−1 and: Ac(i) Bc(i) Ec(i),n Dc(i),n = Bc(i) Ic(i)

(5.92)

The term Dc(i),n in Eq. 5.91 includes the properties of the i-th concrete element introduced at τset while εset−1 deﬁnes the strain diagram at time τset−1 , i.e. immediately prior to the setting of the concrete in the i-th element.

Uncracked sections 203 The cross-sectional rigidities to be used at τj are: RA,j =

mc

Ac(i) Ec(i),j +

i=1

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ec(i),j + RA,s + RA,p

i=1

(5.93a) RB,j =

mc

Bc(i) Ec(i),j +

i=1

=

mc

ms

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ec(i),j + RB,s + RB,p

(5.93b)

i=1

RI,j =

mc

Ic(i) Ec(i),j +

i=1

=

mc

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

i=1

Ic(i) Ec(i),j + RI,s + RI,p

(5.93c)

i=1

and ﬁnally, the stress distributions at τj can be determined from j−1

σc(i),j = Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n n=0 j−1

= Ec(i),j

& ' 1 y εj − εset−1 − εsh(i),j + Fe(i),j,n σc(i),n

(5.94a)

n=0

σs(i),j = Es(i) εj − εs(i),set−1 = Es(i) 1 ys(i) εj − εset−1 σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j − εp(i),set−1 = Ep(i) 1 yp(i) εj − εset−1 + Ep(i) εp(i),init − Ep(i) εp.rel(i),j

(5.94b)

(5.94c)

where εj = εr,j + yκj = 1 y εj .

Example 5.10 The bridge girder with cross-section shown in Fig. 5.20 is subjected to the following load history. The I-section is cast and moist cured for 7 days. At age 7 days, the member is post-tensioned with an initial prestressing force of 2000 kN (Pp,init = 1000 kN in each tendon). The diameter of each prestressing duct is 60 mm. The moment at the cross-section due to the self-weight of the girder is M7 = 550 kNm and is ﬁrst applied to the cross-section during the posttensioning operation at age 7 days. Shrinkage of the concrete in the I-girder also begins to develop at this time. At age 40 days, the slab deck is cast and cured

204 Uncracked sections and the moment caused by the weight of the wet concrete, M40 = 620 kNm, is ﬁrst applied to the precast I-section. The post-tensioning ducts are also grouted at this time (i.e. at age 40 days). Composite action gradually begins to develop as soon as the concrete in the deck sets and the grout within the ducts hardens. Full composite action may not be achieved for several days. However, it is here assumed that the deck and the I-section act compositely and that the prestressing tendons are bonded to the concrete at all times after age 40 days. Shrinkage of the deck is assumed to also begin at age 40 days. At τ = 60 days, the road surface is placed and other superimposed dead loads are applied to the bridge, thereby introducing an additional moment of M60 = 400 kNm. Thereafter, the loads are assumed to remain constant in time. The stress and strain distributions on the cross-section are to be calculated at the following times: (i) immediately after the application of the prestress at age 7 days; (ii) before and after the slab deck is cast at age 40 days; (iii) after the deck and I-section act compositely at age 40 days; (iv) before and after the road surface is placed at age 60 days; (v) at age 30,000 days (i.e. about 80 years) assuming the applied actions acting at age 60 days remain constant thereafter. Based on this loading history the following steps 0 to 6 are considered in the worked example: Step

Age (in days)

0

7

1

40 −

2

40 +

3

40 ++

4

60 −

5

60 +

6

30,000

Description of event Prestressing force applied to the section. Application of M7 = 550 kNm (short-term analysis). Time step introduced to determine the effects of creep, shrinkage and relaxation in the I-girder from age 7 days to age 40 days under the action introduced at 7 days and held constant thereafter (time analysis). The deck is poured introducing an additional moment of M40 = 620 kNm to be resisted by the I-section alone (short-term analysis) Change in cross-section due to grouting of ducts and deck acting compositely with the I-section (from this point in time). Time step introduced to evaluate the time-dependent behaviour of the composite section under constant actions between ages 40 and 60 days (time analysis). Road surface added causing an additional moment of M60 = 400 kNm to be applied to the composite section (short-term analysis). Time step introduced to evaluate the ﬁnal long-term behaviour assuming loads remain constant after age 60 days.

Uncracked sections 205 The material properties are: For all reinforcing steel and tendons: Es = Ep = 200 GPa ϕp (7, σp,init ) = 0 ϕp (40, σp,init ) = 0.015 ϕp (60, σp,init ) = 0.02 ϕp (30,000, σp,init ) = 0.03 For the precast I-section (Concrete element 1): Ec(1),0 = 25 GPa Ec(1),1 = Ec(1),2 = Ec(1),3 = 32 GPa Ec(1),4 = Ec(1),5 = 34 GPa Ec(1),6 = 38 GPa ϕ(1) (7, 7) = 0 ϕ(1) (40, 7) = 0.8 ϕ(1) (60, 7) = 1.0 ϕ(1) (30,000, 7) = 2.5 ϕ(1) (40, 40) = 0 ϕ(1) (60, 40) = 0.8 ϕ(1) (30,000, 40) = 1.8 ϕ(1) (60, 60) = 0 ϕ(1) (30,000, 60) = 1.6 εsh(1) (7) = 0 εsh(1) (40) = −100 × 10−6 εsh(1) (60) = −150 × 10−6 εsh(1) (30,000) = −400 × 10−6 For the concrete deck (Concrete element 2): Ec(2),3 = 18 GPa Ec(2),4 = Ec(2),5 = 25 GPa Ec(2),6 = 30 GPa

206 Uncracked sections ϕ(2) (40, 40) = 0 ϕ(2) (60, 40) = 2.0 ϕ(2) (30,000, 40) = 3.5 ϕ(2) (60, 60) = 0 ϕ(2) (30,000, 60) = 2.8 εsh(2) (40) = 0 εsh(2) (60) = −200 × 10−6 εsh(1) (30,000) = −600 × 10−6 As for Example 5.9, the top ﬁbre of the concrete deck is selected as the reference axis, i.e. dref = 0 mm, and the distances of the steel and prestressing layers from the reference axis are ys(1) = 75 mm, ys(2) = 210 mm, ys(3) = 1240 mm, yp(1) = 1030 mm and yp(2) = 1160 mm. The external loads applied at each step are: 0N re,0 = re,1 = 550 × 106 Nmm

0N re,2 = re,3 = re,4 = 1170 × 106 Nmm

0N re,5 = re,6 = 1570 × 106 Nmm

The concrete material coefﬁcients to be used in the various analyses are as follows: For the precast I-section (Element 1): Jc(1) (7, 7) = 4 × 10−5 MPa−1 Jc(1) (40, 7) = 7.2 × 10−5 MPa−1 Jc(1) (60, 7) = 8 × 10−5 MPa−1 Jc(1) (30,000, 7) = 14 × 10−5 MPa−1 Jc(1) (40, 40) = 3.125 × 10−5 MPa−1 Jc(1) (60, 40) = 5.625 × 10−5 MPa−1 Jc(1) (30,000, 40) = 8.75 × 10−5 MPa−1 Jc(1) (60, 60) = 2.941 × 10−5 MPa−1 Jc(1) (30,000, 60) = 7.647 × 10−5 MPa−1

Uncracked sections 207 Jc(1) (30,000, 30,000) = 2.631 × 10−5 MPa−1 Fe(1),1,0 = Fe(1),2,0 = Fe(1),3,0 = −1.304 Fe(1),4,0 = Fe(1),5,0 = −0.807 Fe(1),6,0 = −1.995 Fe(1),4,3 = Fe(1),5,3 = −0.912 Fe(1),6,3 = −0.419 Fe(1),6,5 = −1.906 Fe(1),i,j = 0 if τi = τj εsh(1) (7) = 0 εsh(1) (40) = εsh(1),1 = εsh(1),2 = εsh(1),3 = −100 × 10−6 εsh(1) (60) = εsh(1),4 = εsh(1),5 = −150 × 10−6 εsh(1) (30,000) = εsh(1),6 = −400 × 10−6 For the concrete deck (Element 2): Jc(2) (40, 40) = 5.555 × 10−5 MPa−1 Jc(2) (60, 40) = 16.66 × 10−5 MPa−1 Jc(2) (30,000, 40) = 25 × 10−5 MPa−1 Jc(2) (60, 60) = 4.0 × 10−5 MPa−1 Jc(2) (30,000, 60) = 15.2 × 10−5 MPa−1 Jc(2) (30,000, 30,000) = 3.333 × 10−5 MPa−1 Fe(2),4,3 = Fe(2),5,3 = −3.166 Fe(2),6,3 = −2.94 Fe(2),6,5 = −3.56 Fe(2),i,j = 0 if τi = τj εsh(2) (40) = εsh(2),1 = εsh(2),2 = εsh(2),3 = 0 εsh(2) (60) = εsh(2),4 = εsh(2),5 = −200 × 10−6 εsh(2) (30,000) = εsh(2),6 = −600 × 10−6 The initial prestress is included in the analysis using: 2000 × 103 N fp,init = 2190 × 106 Nmm

208 Uncracked sections The concrete area of the I-section contributing to the cross-sectional rigidity changes when the prestressing ducts are grouted. For clarity, the concrete properties of the I-section before grouting are referred to as Ac(1a) , Bc(1a) and Ic(1a) , and after grouting as Ac(1b) , Bc(1b) and Ic(1b) . The procedures required to analyse the I-section in the ﬁrst three steps (before the concrete deck is cast) are identical to those illustrated in Examples 5.2 and 5.6 and, for this reason, only the results of the analyses for Steps 1, 2 and 3 are presented here.

Step 0: Short-term analysis at age τ = 7 days Concrete properties: Ac(1a) = 308.6 × 103 mm2 ; Bc(1a) = 229.7 × 106 mm3 ; and Ic(1a) = 219.5 × 109 mm4 . Cross-sectional rigidities: RA,0 = 8256 × 106 N; RB,0 = 6228 × 109 Nmm; and RI,0 = 6050 × 1012 Nmm2 . The matrix F0 : F0 =

542.2 × 10−12 N−1

−558.2 × 10−15 N−1 mm−1

−558.2 × 10−15 N−1 mm−1

739.9 × 10−18 N−1 mm−2

Strain at reference axis and curvature: εr,0 = −169.0 × 10−6 and κ0 = −0.097 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε0(top) = −183.6 × 10−6 and ε0(btm) = −295.2 × 10−6 . Concrete stresses: σc(1),0(top) = −4.60 MPa and σc(1),0(btm) = −7.38 MPa. Reinforcement stresses: σs(2),0 = −37.9 MPa and σs(3),0 = −57.9 MPa. Stresses in tendons: σp(1),0 = 1250 MPa and σp(2),0 = 1250 MPa. The concrete stress resultants at τ0 = 7 days are: −1862 × 103 N . rc(1),0 = −1504 × 106 Nmm

Step 1: Time analysis – SSM at age τ1 = 40 days Creep and shrinkage of the concrete as well as relaxation of the prestressing steel in the I-section are accounted for with: fcr,1 =

2427 × 103 N

1961 × 106 Nmm

fsh,1 =

−987.7 × 103 N

−735.3 × 106 Nmm

fp.rel,1 =

30 × 103 N

32.85 × 106 Nmm

Uncracked sections 209 Cross-sectional rigidities: RA,1 = 10416 × 106 N; RB,1 = 7837 × 109 Nmm; and 12 Nmm2 . RI,1 = 7587 × 10 The matrix F1 =

430.7 × 10−12 N−1

−444.8 × 10−15 N−1 mm−1

−444.8 × 10−15 N−1 mm−1

591.3 × 10−18 N−1 mm−2

.

Strain at reference axis and curvature: εr,1 = −405.1 × 10−6 and κ1 = −0.148 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε1(top) = −427.4 × 10−6 and ε1(btm) = −598.5 × 10−6 . Concrete stresses: σc(1),1(top) = −4.49 MPa and σc(1),0(btm) = −6.33 MPa. Reinforcement stresses: σs(2),1 = −87.3 MPa and σs(3),1 = −117.9 MPa. Stresses in tendons: σp(1),1 = 1231 MPa and σp(2),1 = 1231 MPa. The concrete stress resultants at τ1 = 40 days are: −1679 × 103 N . rc(1),1 = −1327 × 106 Nmm

Step 2: Short-term analysis at age τ = 40 days This step is identical to the previous one with the exception that the applied external load has increased due to the pour of the concrete deck. Strain at reference axis and curvature: εr,2 = −680.9 × 10−6 and κ2 = 0.217 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε2(top) = −648.2 × 10−6 and ε2(btm) = −397.7 × 10−6 . Concrete stresses: σc(1),2(top) = −11.56 MPa and σc(1),2(btm) = 0.09 MPa. Reinforcement stresses: σs(2),2 = −127.0 MPa and σs(3),2 = −82.1 MPa. Stresses in tendons: σp(1),2 = 1231 MPa and σp(2),2 = 1231 MPa. The concrete stress resultants at τ = 40 days after the wet concrete is poured are: −1708 × 103 N . rc(1),2 = −779.8 × 106 Nmm

Step 3: Grouting of tendons and commencement of composite action at age τ1 = 40 days During this step, the cross-sectional properties change due to the grouting of the tendons and due to the deck beginning to act compositely with the I-section. This change in cross-section will be captured in f set,j to ensure that the added components are unloaded at the time of setting. The cross-sectional properties of both I-section (element 1) and the concrete deck (element 2) are: Ac(1b) = 312.7 × 103 mm2 Bc(1b) = 234.2 × 106 mm3 Ic(1b) = 224.4 × 109 mm4

210 Uncracked sections Ac(2) = 357.3 × 103 mm2 Bc(2) = 26.79 × 106 mm3 Ic(2) = 2685 × 106 mm4 The cross-sectional rigidities are: RA,3 = 17,840 × 106 N RB,3 = 8852 × 109 Nmm; and RI,3 = 8179 × 1012 Nmm2 Matrix F3 is now: F3 =

121.1 × 10−12 N−1

−131.0 × 10−15 N−1 mm−1

−131.0 × 10−15 N−1

264.1 × 10−18 N−1 mm−1

The time-dependent effects of creep and shrinkage of the concrete and the relaxation response, that is, f cr,3 , f sh,3 and f p.rel,3 , are identical to those of the previous two steps as they all correspond to age 40 days. The vectors deﬁning the unloaded condition for the grout, prestressing and concrete deck at the time of setting are determined below. For prestressing cables and grout: Agrout = Aduct(1) + Aduct(2) − Apre(1) − Apre(2) = 2827 + 2827 − 800 − 800 = 4054 mm2 Bgrout = Bduct(1) + Bduct(2) − Bpre(1) − Bpre(2) = (2827 − 800) × 1030 + (2827 − 800) × 1160 = 4439.1 × 103 mm3 Igrout = Iduct(1) + Iduct(2) − Ipre(1) − Ipre(2) = (2827 − 800) × 10302 + (2827 − 800) × 11602 = 4877.9 × 106 mm4

Agrout Ec(1),3 εr,2 + Bgrout Ec(1),3 κ2 fc(1).set,3 = Bgrout Ec(1),3 εr,2 + Igrout Ec(1),3 κ2 ⎤ ⎡ 4054 × 32,000 × −680.9 × 10−6 + 4439.1 × 103 ⎥ ⎢ ⎥ ⎢ ×32,000 × 0.217 × 10−6 ⎥ ⎢ =⎢ ⎥ ⎣4439.1 × 103 × 32,000 × −680.9 × 10−6 + 4877.9 × 106 ⎦ ×32,000 × 0.217 × 10−6 −57.4 × 103 N = −62.7 × 106 Nmm

Uncracked sections 211

Ap(1) Ep(1) εr,2 + Bp(1) Ep(1) κ2 Bp(1) Ep(1) εr,2 + Ip(1) Ep(1) κ2 ⎤ ⎡ 800 × 200 × 103 × −680.9 × 10−6 + 800 × 1030 ⎥ ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎢ ⎥ =⎢ ⎥ 3 −6 2 + 800 × 1030 × −680.9 × 10 800 × 1030 × 200 × 10 ⎣ ⎦ ×200 × 103 × 0.217 × 10−6 −73.0 × 103 N = −75.2 × 106 Nmm Ap(2) Ep(2) εr,2 + Bp(2) Ep(2) κ2 fp(2).set,3 = Bp(2) Ep(2) εr,2 + Ip(2) Ep(2) κ2 ⎡ ⎤ 800 × 200 × 103 × −680.9 × 10−6 + 800 × 1160 ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎥ ⎥ =⎢ ⎢ ⎥ ⎣800 × 1160 × 200 × 103 × −680.9 × 10−6 + 800 × 11602 ⎦ ×200 × 103 × 0.217 × 10−6 −68.5 × 103 N = −79.5 × 106 Nmm

fp(1).set,3 =

For the concrete deck: Ac(2) Ec(2),3 εr,2 + Bc(2) Ec(2),3 κ2 fc(2),set,3 = Bc(2) Ec(2),3 εr,2 + Ic(2) Ec(2),3 κ2 ⎡ ⎤ 357,300 × 18,000 × −680.9 × 10−6 + 26.79 × 106 ⎢ ⎥ ⎢ ×18,000 × 0.217 × 10−6 ⎥ ⎢ ⎥ =⎢ ⎥ 6 −6 6 + 2685 × 10 ⎦ ⎣26.79 × 10 × 18,000 × −680.9 × 10 ×18,000 × 0.217 × 10−6 −4274 × 103 N = −317.9 × 106 Nmm As(1) Es(1) εr,2 + Bs(1) Es(1) κ2 fs(1).set,3 = Bs(1) Es(1) εr,2 + Is(1) Es(1) κ2 ⎤ ⎡ 2700 × 200 × 103 × −680.9 × 10−6 + 202.5 × 103 ⎥ ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎢ ⎥ =⎢ ⎥ 3 3 −6 6 + 15.19 × 10 × 200 × 10 × −680.9 × 10 202.5 × 10 ⎣ ⎦ ×200 × 103 × 0.217 × 10−6 −358.8 × 103 N = −26.9 × 106 Nmm

212 Uncracked sections Combining the above contributions related to concrete setting: fset,3 = fc(1).set,3 + fp(1).set,3 + fp(2).set,3 + fc(2).set,3 + fs(1).set,3 −4832 × 103 N = −562.2 × 106 Nmm The strain distribution at time τ3 can then be determined as: ε3 = F3 re,3 − fcr,3 + fsh,3 − fp,init + fp.rel,3 + fset,3 0 121.1 × 10−12 −131.0 × 10−15 = × 1170 × 106 −131.0 × 10−15 264.1 × 10−18 2427 × 103 −987.7 × 103 2000 × 103 30 × 103 − + − + 1961 × 106 −735.3 × 106 2190 × 106 32.85 × 106 −4832 × 103 −680.9 × 10−6 + = −562.2 × 106 0.217 × 10−6 mm−1 As expected there is no change in deformation between steps 3 and 4 as the new cross-sectional components are kept unloaded. The strain diagram for the precast I-section at step 3 is identical to the one already calculated for step 2: ε3(top) = ε2(top) = −648.2 × 10−6 ε3(btm) = ε2(btm) = −397.7 × 10−6 Stresses at step 3 are also identical to those obtained at Step 2 as shown below: For the precast I-section: " # 1 yc(1),(top) ε3 − εsh(1),3 + Fe(1),3,0 σc(1),0(top) σc(1),3(top) = Ec(1),3 ! −680.9 × 10−6 = 32,000 1 150 − −100 × 10−6 0.217 × 10−6 − 1.304 × (−4.60) = −11.56 MPa " # 1 yc(1),(btm) ε3 − εsh(1),3 + Fe(1),3,0 σc(1),0(btm) σc(1),3(btm) = Ec(1),3 = 0.09 MPa For the concrete deck:

" # 1 yc(2),(top) ε3 − εsh(2),3 − Ec(2),3 1 yc(2),(top) ε2 ! −680.9 × 10−6 = 18,000 1 0 −0 0.217 × 10−6 ! −680.9 × 10−6 − 18,000 1 0 = 0.0 MPa 0.217 × 10−6

σc(2),3(top) = Ec(2),3

Uncracked sections 213 " # σc(2),3(btm) = Ec(2),3 1 yc(2),(btm) ε3 − εsh(2),3 − Ec(2),3 1 yc(2),(btm) ε2 = 0.0 MPa For the non-prestressed reinforcement:

3

σs(1),3 = 200 × 10 × 1 75

−680.9 × 10−6

−

0.217 × 10−6

−680.9 × 10−6

0.217 × 10−6

= 0.0 MPa

−680.9 × 10−6 σs(2),3 = 200 × 10 × 1 210 0.217 × 10−6

3

= −127.0 MPa

−680.9 × 10−6 σs(3),3 = 200 × 10 1 1240 0.217 × 10−6 3

= −82.1 MPa For the prestressing steel: σp(1),3 = Ep(1) 1 yp(1) (ε3 − ε2 ) + Ep(1) (εp(1),init − εp.rel(1),3 ) = 1231 MPa σp(2),3 = Ep(2) 1 yp(2) (ε3 − ε2 ) + Ep(2) (εp(2),init − εp.rel(2),3 ) = 1231 MPa The concrete stress resultants at step 3, τ = 40 days after the wet concrete has set, are: rc(1),3 = Dc(1),3 ε3 + fcr(1),3 − fsh(1),3 − fset(1),3 = rc(2),3 = Dc(2),3 ε3 + fcr(2),3 − fsh(2),3 − fset(2),3 =

−1708 × 103 N

−779.8 × 106 Nmm 0N 0 Nmm

Step 4: Time analysis SSM at age 60 days In step 4, the stresses and strains due to the previous loading history are evaluated at 60 days. The following cross-sectional properties are calculated for step 4: RA,4 = 20,960 × 106 N; RB,4 = 9508 × 109 Nmm; RI,4 = 8647 × 1012 Nmm2 .

214 Uncracked sections The matrix F4 is: F4 =

95.15 × 10−12 N−1

−104.6 × 10−15 N−1 mm−1

−104.6 × 10−15 N−1 mm−1

230.7 × 10−18 N−1 mm−2

The effects of creep and shrinkage in this time period are: fcr,4 = Fe(1),4,0 rc(1),0 + Fe(1),4,3 rc(1),3 −1862 × 103 −1708 × 103 = −0.807 × − 0.912 × −1504 × 106 −779.8 × 106 3061 × 103 N = 1925 × 106 Nmm

Ac(1) Ac(2) fsh,4 = Ec(1),4 εsh(1),4 + Ec(2),4 εsh(2),4 Bc(1) Bc(2)

357,300 312,700 −6 = × 34,000 × −150 × 10 + 234.2 × 106 26.79 × 106 × 25,000 × −200 × 10−6 −1786 × 103 −1595 × 103 −3381 × 103 N = + = −1328 × 106 Nmm −1195 × 106 −133.9 × 106 Note that the grout is assumed to be shrinking at the same rate as the concrete used for the precast I-section. The effects of relaxation of the steel tendon are calculated from Eq. 5.90f: fp.rel,4 =

Ap(1) Ep(1) εp(1),init ϕp (60, σp(1),init )

yp(1) Ap(1) Ep(1) εp(1),init ϕp (60, σp(1),init ) Ap(2) Ep(2) εp(2),init ϕp (60, σp(2),init ) 40 × 103 N + = yp(2) Ap(2) Ep(2) εp(2),init ϕp (60, σp(2),init ) 43.8 × 106 Nmm

The terms deﬁning f set,4 are calculated based on the corresponding values already obtained at time τ3 and adjusted for the change in elastic moduli that has taken place: −57.4×103 34,000 −61.0×103 N Ec(1),4 fc(1).set,4 = fc(1).set,3 = = Ec(1),3 −66.6×106 Nmm −62.7×106 32,000 −73.0×103 N fp(1).set,4 = fp(1).set,3 = −75.2×106 Nmm

fp(2).set,4 = fp(2).set,3 =

−68.5 × 103

−79.5 × 106

N

Uncracked sections 215

Nmm

−4274 × 103 Ec(2),4 = fc(2).set,4 = fc(2).set,3 Ec(2),3 −317.9 × 106 −5936 × 103 N = −441.5 × 106 Nmm −358.8 × 103 N fs(1).set,4 = fs(1).set,3 = −26.9 × 106 Nmm

25,000 18,000

fset,4 = fc(1).set,4 + fp(1).set,4 + fp(2).set,4 + fc(2).set,4 + fs(1).set,4 −6498 × 103 N = −689.8 × 106 Nmm The strain distribution at time τ4 becomes: ε4 = F4 re,4 − fcr,4 + fsh,4 − fp,init + fp.rel,4 + fset,4 0 95.15 × 10−12 −104.6 × 10−15 = × 1170 × 106 −104.6 × 10−15 230.7 × 10−18 3061 × 103 −3381 × 103 2000 × 103 40 × 103 − + − + 1925 × 106 −1328 × 106 2190 × 106 43.8 × 106 −6498 × 103 −903.0 × 10−6 + = −689.8 × 106 0.424 × 10−6 mm−1 At age 60 days, εr,4 = −903.0 × 10−6 and κ4 = 0.424 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to: ε4(top) = εr,4 + 150 × κ4 = −839.4 × 10−6 and ε4(btm) = εr,4 + 1300 × κ4 = −351.9 × 10−6 Stresses at the end of step 4 are calculated below: For the precast I-section: " # 1 yc(1),(top) ε4 − εsh(1),4 + Fe(1),4,0 σc(1),0(top) σc(1),4(top) = Ec(1),4 + Fe(1),4,3 σc(1),3(top) ! −903.0 × 10−6 −6 − −150 × 10 = 34,000 1 150 0.424 × 10−6 − 0.807 × (−4.60) − 0.912 × (−11.56) = −9.19 MPa

216 Uncracked sections and σc(1),4(btm) = Ec(1),4

" # 1 yc(1),(btm) ε4 − εsh(1),4 + Fe(1),4,0 σc(1),0(btm)

+ Fe(1),4,3 σc(1),3(btm) = −0.99 MPa For the concrete deck: " # 1 yc(2),(top) (ε4 − ε2 ) + Fe(2),4,3 σc(1),3(top) − εsh(2),4 −903.0 × 10−6 −680.9 × 10−6 = 25,000 1 0 − +0 0.424 × 10−6 0.217 × 10−6 ! − −200 × 10−6 = −0.55 MPa

σc(2),4(top) = Ec(2),4

" # 1 yc(2),(btm) (ε4 − ε2 ) + Fe(2),4,3 σc(1),3(btm) − εsh(2),4 −903.0 × 10−6 −680.9 × 10−6 = 25,000 1 150 − +0 0.424 × 10−6 0.217 × 10−6 ! −6 = 0.22 MPa − −200 × 10

σc(2),4(btm) = Ec(2),4

For the non-prestressed reinforcement: 3

σs(1),4 = 200 × 10 × 1 75

−903.0 × 10−6 0.424 × 10−6

−

−680.9 × 10−6 0.217 × 10−6

= −41.3 MPa

−903.0 × 10−6 σs(2),4 = 200 × 10 × 1 210 = −162.8 MPa 0.424 × 10−6 −6 −903.0 × 10 σs(3),4 = 200 × 103 1 1240 = −75.5 MPa 0.424 × 10−6 3

For the prestressing steel: σp(1),4 = Ep(1) 1 yp(1) (ε4 − ε2 ) + Ep(1) εp(1),init − εp.rel(1),4 −903.0 × 10−6 −680.9 × 10−6 3 = 200 × 10 × 1 1030 − 0.424 × 10−6 0.217 × 10−6 + 200,000 × 0.00625 × (1 − 0.02) = 1223 MPa

Uncracked sections 217 σp(2),4 = Ep(2) 1 yp(2) (ε4 − ε2 ) + Ep(2) εp(2),init − εp.rel(2),4 −6 −6 −680.9 × 10 −903.0 × 10 = 200 × 103 × 1 1160 − 0.424 × 10−6 0.217 × 10−6

+ 200,000 × 0.00625 × (1 − 0.02) = 1228 MPa The concrete stress resultants at step 4 at τ = 60 days are: rc(1),4 = Dc(1),4 ε4 + fcr(1),4 − fsh(1),4 − fc(1).set,4 312,700 234.2 × 106 −903.0 × 10−6 = 34,000 × 0.424 × 10−6 234.2 × 106 224.4 × 109 3061 × 103 −1595 × 103 −61.0 × 103 + − − 1925 × 106 −1195 × 106 −66.6 × 106 −1507 × 103 N = −769.1 × 106 Nmm rc(2),4 = Dc(2),3 ε4 + fcr(2),4 − fsh(2),4 − fc(2).set,4 −903.0 × 10−6 357,300 26.79 × 106 0 + = 25,000 × 6 −6 6 0 0.424 × 10 26.79 × 10 2685 × 10 −1786 × 103 −5936 × 103 −59.7 × 103 N − − = −0.999 × 106 Nmm −133.9 × 106 −441.5 × 106

Step 5: Time analysis SSM at age 60 days The cross-sectional properties, the creep and shrinkage of the concrete and relaxation of the prestressing tendons are identical to the previous step. The only change for step 5 is an additional external moment applied to the composite section. Based on the results calculated for step 4, the strain variables can be calculated by modifying vector re,5 to account for the change in external moment as: ε5 = F5 re,5 − fcr,5 + fsh,5 − fp,init + fp.rel,5 + fset,5 0 95.15 × 10−12 −104.6 × 10−15 = × 1570 × 106 −104.6 × 10−15 230.7 × 10−18 3061 × 103 −3381 × 103 2000 × 103 40 × 103 − + − + 1925 × 106 −1328 × 106 2190 × 106 43.8 × 106 −6498 × 103 −944.9 × 10−6 + = −689.8 × 106 0.516 × 10−6 mm−1

218 Uncracked sections At age 60 days, after the application of the road deck and other imposed dead loads, εr,5 = −944.9 × 10−6 and κ5 = 0.516 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to: ε5(top) = εr,5 + 150 × κ5 = −867.4 × 10−6 and ε5(btm) = εr,5 + 1300 × κ5 = −273.8 × 10−6 Stresses at the end of step 5 are calculated below: For the precast I-section: " # 1 yc(1),(top) ε5 − εsh(1),5 + Fe(1),5,0 σc(1),0(top) σc(1),5(top) = Ec(1),5 + Fe(1),5,3 σc(1),3(top) ! −944.9 × 10−6 = 34,000 1 150 − −150 × 10−6 0.516 × 10−6 − 0.807 × (−4.60) − 0.912 × (−11.56) = −10.14 MPa and σc(1),5(btm) = Ec(1),5

" # 1 yc(1),(btm) ε5 − εsh(1),5 + Fe(1),5,0 σc(1),0(btm)

+ Fe(1),5,3 σc(1),3(btm) = 1.66 MPa For the concrete deck:

" # 1 yc(2),(top) (ε5 − ε2 ) + Fe(2),5,3 σc(1),3(top) − εsh(2),5 −944.9 × 10−6 −680.9 × 10−6 = 25,000 1 0 − +0 0.516 × 10−6 0.217 × 10−6 ! −6 − −200 × 10 = −1.60 MPa

σc(2),5(top) = Ec(2),5

and σc(2),5(btm) = Ec(2),5

" # 1 yc(2),(btm) (ε5 − ε2 ) + Fe(2),5,3 σc(1),3(btm) − εsh(2),5

= −0.48 MPa For the non-prestressed reinforcement: −944.9 × 10−6 −680.9 × 10−6 3 σs(1),5 = 200 × 10 × 1 75 − 0.516 × 10−6 0.217 × 10−6 = −48.3 MPa

Uncracked sections 219

−944.9 × 10−6 σs(2),5 = 200 × 103 × 1 210 = −167.3 MPa 0.516 × 10−6 −944.9 × 10−6 3 σs(3),5 = 200 × 10 1 1240 = −60.9 MPa 0.516 × 10−6 For the prestressing steel: σp(1),5 = Ep(1) 1 yp(1) (ε5 − ε2 ) + Ep(1) εp(1),init − εp.rel(1),5 −944.9 × 10−6 −680.9 × 10−6 3 = 200 × 10 × 1 1030 − 0.516 × 10−6 0.217 × 10−6 + 200,000 × 0.00625 × (1 − 0.02) = 1234 MPa σp(2),5 = Ep(2) 1 yp(2) (ε5 − ε2 ) + Ep(2) εp(2),init − εp.rel(2),5 = 1241 MPa The concrete stress resultants at step 5 at τ = 60 days are: rc(1),5 = Dc(1),5 ε5 + fcr(1),5 − fsh(1),5 − fc(1).set,5 312,700 234.2 × 106 −944.9 × 10−6 = 34,000 × 0.516 × 10−6 234.2 × 106 224.4 × 109 3061 × 103 −1595 × 103 −61.0 × 103 + − − 1925 × 106 −1195 × 106 −66.6 × 106 −1217 × 103 N = −398.3 × 106 Nmm rc(2),5 = Dc(2),5 ε5 + fcr(2),5 − fsh(2),5 − fc(2).set,5 357,300 26.79 × 106 −944.9 × 10−6 0 = 25,000 × + 6 6 −6 0 0.516 × 10 26.79 × 10 2685 × 10 −1786 × 103 −5936 × 103 −371.7 × 103 N − − = −22.8 × 106 Nmm −133.9 × 106 −441.5 × 106

Step 6: Time analysis – SSM at age 30,000 days The cross-sectional rigidities for step 6 are: RA,6 = 24,000 × 106 N; RB,6 = 10,580 × 109 Nmm; RI,6 = 9558 × 1012 Nmm2 .

220 Uncracked sections The matrix F6 is: F6 =

81.35 × 10−12 N−1

−90.03 × 10−15 N−1 mm−1

−90.03 × 10−15 N−1 mm−1

204.2 × 10−18 N−1 mm−2

The effects of creep and shrinkage in this time period are: fcr,6 = Fe(1),6,0 rc(1),0 + Fe(1),6,3 rc(1),3 + Fe(1),6,5 rc(1),5 + Fe(2),6,5 rc(2),5 −1862 × 103 −1708 × 103 = −1.995 × − 0.419 × −1504 × 106 −779.8 × 106 −1217 × 103 −371.7 × 103 − 1.906 × − 3.56 × −398.3 × 106 −22.8 × 106 8074 × 103 N = 4167 × 106 Nmm

Ac(2) Ac(1) fsh,6 = Ec(1),6 εsh(1),6 + Ec(2),6 εsh(2),6 Bc(1) Bc(2) 357,300 312,700 −6 × 38,000 × −400 × 10 + = 26.79 × 106 234.2 × 106 × 30,000 × −600 × 10−6 −11,180 × 103 N = −4042 × 106 Nmm Relaxation of the steel tendon is accounted for using: fp.rel,6 =

2

Ap(i) Ep(i) εp(i),init ϕp (30,000, σp(i),init )

yp(i) Ap(i) Ep(i) εp(i),init ϕp (30,000, σp(i),init ) 800 × 200,000 800 × 200,000 = + 1030 × 800 × 200,000 1160 × 800 × 200,000 60.0 × 103 N × 0.00625 × 0.030 = 65.7 × 106 Nmm i=1

The terms deﬁning f set,6 are calculated using the same procedure adopted at time τ4 : −57.4 × 103 38,000 −68.1 × 103 N Ec(1),6 = = fc(1).set,6 = fc(1).set,3 Ec(1),3 −74.5 × 106 Nmm −62.7 × 106 32,000

fp(1).set,6 = fp(1).set,3 =

N

Uncracked sections 221

−75.2 × 106

fp(2).set,6 = fp(2).set,3 =

−73.0 × 103

Nmm −68.5 × 103 N

−79.5 × 106 Nmm −4274 × 103 30,000 Ec(2),6 fc(2).set,6 = fc(2).set,3 = Ec(2),3 −317.9 × 106 18,000 −7123 × 103 N = −529.8 × 106 Nmm −358.8 × 103 N fs(1).set,6 = fs(1).set,3 = −26.9 × 106 Nmm fset,6 = fc(1).set,6 + fp(1).set,6 + fp(2).set,6 + fc(2).set,6 + fs(1).set,6 −7692 × 103 N = −785.9 × 106 Nmm

The strain distribution at time τ6 becomes: ε6 = F6 re,6 − fcr,6 + fsh,6 − fp,init + fp.rel,6 + fset,6 0 81.35 × 10−12 −90.03 × 10−15 = × 1570 × 106 −90.03 × 10−15 204.2 × 10−18 8074 × 103 −11,180 × 103 2000 × 103 60.0 × 103 − + − + 4167 × 106 −4042 × 106 2190 × 106 65.7 × 106 −7692 × 103 −1490 × 10−6 + = −785.9 × 106 0.650 × 10−6 mm−1 At age 30,000 days, εr,6 = −1490 × 10−6 and κ6 = 0.650 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to ε6(top) = −1393 × 10−6 and ε6(btm) = −644.8 × 10−6 . The strains in the top and bottom of the concrete deck are calculated as follows (measured from the time of setting): ε6,(top) = 1 0 (ε6 − ε2 ) = −809.5 × 10−6 ε6,(btm) = 1 150 (ε6 − ε2 ) = −744.6 × 10−6 Final stresses at time 30,000 days are calculated below: For the precast I-section: σc(1),6(top) = −4.40 MPa; σc(1),6(btm) = 2.21 MPa For the concrete deck: σc(2),6(top) = −0.59 MPa; σc(2),6(btm) = −2.63 MPa

222 Uncracked sections For the non-prestressed reinforcement: σs(1),6 = −155.4 MPa; σs(2),6 = −270.8 MPa; σs(3),6 = −136.8 MPa For the prestressing steel: σp(1),6 = 1140 MPa; σp(2),6 = 1151 MPa. The strains and stresses at times τ0 and τ6 are plotted in Fig. 5.22. −183.6

−4.60 −37.9

1250 1250

−57.9 −295.2 −7.38 Strain × 10−6 Stress (MPa) (a) Cross-section −427.4

(b) Step 0: At 7 days −648.9

−4.49

−11.56

−87.3

−127.0 1231

1231 −82.1

−117.9

1231 −6.33 Stress (MPa)

−598.5 Strain × 10−6

(c) Step 1: Age 40 days before slab deck is cast −222.1 −839.4 −191.2 −9.19

−0.55 −41.3

−162.8

−397.7 Strain × 10−6

1231 0.09 Stress (MPa)

(d) Steps 2 and 3: Age 40 days after deck is cast and tendons are grouted −264.0 −1.60 −867.4 −219.2 −10.14 −48.3 −167.3

0.22

1234

1223 −60.9

−75.5 −351.9 Strain × 10−6

1228 −0.99 Stress (MPa)

−273.8 Strain × 10−6

−809.5 −744.6

1241 1.66 Stress (MPa)

(f) Step 5: Age 60 days after road surface applied

(e) Step 4: Age 60 days before road surface applied −1393

−0.48

−155.4 −4.40 −270.8

−0.59 −2.63

1140 −136.8

1151 −644.8 2.21 Stress (MPa) Strain × 10−6 (g) Step 6: Age 30,000 days

Figure 5.22 Strain and stress distributions for Example 5.10.

Uncracked sections 223

5.8 References 1. Gilbert, R.I. (1988). Time Effects in Concrete Structures. Elsevier Science Publishers, Amsterdam. 2. Ghali, A., Favre, R. and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London. 3. Standards Australia (2004). Australian Standard for Bridge Design – Part 5: Concrete (AS5100.5–2004). Sydney, Australia. 4. Bazant, Z.P. and Wu, S.T. (1973). Dirichlet series creep function for aging concrete. Journal of the Engineering Mechanics Division, ASCE, 99(2), 367–387. 5. Bazant, Z.P. and Wu, S.T. (1974). Rate-type creep law of aging concrete based on Maxwell chain. Materials and Structures (RILEM), 7(37), 45–60. 6. Bradford, M.A. and Gilbert, R.I. (1992). Composite beams with partial interaction under sustained loads. Journal of Structural Engineering, ASCE, 118(7), 1871–1883. 7. Tarantino, A.M. and Dezi, L. (1992). Creep effects in composite beams with ﬂexible shear connectors. Journal of Structural Engineering, ASCE, 118(8), 2063–2081. 8. Dezi, L. and Tarantino, A.M. (1993). Creep in composite continuous beams-I: theoretical treatment. Journal of Structural Engineering, ASCE, 119(7), 2095–2111. 9. Gilbert, R.I. and Bradford, M.A. (1995). Time-dependent behaviour of continuous composite beams at service loads. Journal of Structural Engineering, ASCE, 121(2), 319–327. 10. Ranzi, G. and Bradford, M.A. (2006). Analytical solutions for the time-dependent behaviour of composite beams with partial interaction. International Journal of Solids and Structures, 43, 3770–3793. 11. Ranzi, G. and Bradford, M.A. (2009). Analysis of composite beams with partial interaction using the direct stiffness approach for time effects. International Journal for Numerical Methods in Engineering, 78, 564–586.

6

Uncracked sections Axial force and biaxial bending

6.1 Introduction Methods of analysis to evaluate the short- and long-term response of concrete crosssections subjected to axial force and biaxial bending are presented in this chapter. These methods are particularly useful for the analysis of reinforced, prestressed or composite steel-concrete columns in building structures. The concrete is assumed to remain uncracked and be able to carry any applied tension. The proposed formulation relies on the Euler–Bernoulli beam assumptions which require plane sections to remain plane and perpendicular to the member axis before and after deformation. As for the case of axial loading and uniaxial bending (Chapter 5), the governing system of equations describing the structural response is expressed as a function of the unknown variables required to deﬁne the strain diagram. For the case of biaxial bending, the strain diagram is deﬁned in terms of three variables, speciﬁcally the strain measured at the origin of the adopted orthogonal co-ordinate system εr and the curvatures calculated with respect to the two orthogonal x- and y-axes, κx and κy , respectively (as illustrated in Fig. 6.1). The external actions applied to the cross-section may include an axial force applied at the origin Ne and bending moments Mxe and Mye applied with respect to the x- and y-axes, respectively. As shown in Fig. 6.1b, the ﬂexural action is equivalent to an external moment Me applied at an angle θM . The strain at an arbitrary point on the cross-section can be calculated from: ε = εr + yκx − xκy

(6.1)

The negative sign placed before the third term in Eq. 6.1 is a consequence of the sign convention adopted for the applied moments (as illustrated in Fig. 6.1b). The three variables deﬁning the strain diagrams, i.e. εr , κx and κy , are determined by enforcing horizontal and rotational equilibrium on the cross-section: Ne = Ni

(6.2a)

Mxe = Mxi

(6.2b)

Mye = Myi

(6.2c)

Uncracked sections 225 er x

e kx

y

qM

x Mxe

y x

er

y

ky e (a) Generic cross-section and strain diagram

Me

Mye

(b) Applied moments

Figure 6.1 Typical section, strain distribution and sign convention for applied moments.

where Ni , Mxi and Myi are the internal actions resisted by the cross-section, i.e. axial force and moments with respect to the x- and y-axes, respectively, and are deﬁned as: (6.3a) Ni = σ dA A

Mxi =

yσ dA A

(6.3b)

Myi = −

xσ dA

(6.3c)

A

The negative sign included in the expression for Myi has been introduced to match the sign convention adopted for the external moment Mye (see Fig. 6.1b). It is useful to evaluate the angle of inclination θM of the applied moment Me measured from the x-axis (adopting clockwise rotations to be positive) using: tan θM =

Mye Mxe

(6.4)

The values of the three unknowns (εr , κx and κy ) are obtained by enforcing equilibrium (Eq. 6.2), with the strain over the section expressed by Eq. 6.1 (i.e. strain compatibility) and using the appropriate constitutive relationships in the calculation of the internal stresses and actions. For ease of notation, the derivations presented in the following are applicable to generic reinforced and prestressed concrete cross-sections, while other types of crosssections could be easily considered, for example, the composite sections considered in Chapter 5. The reinforced or prestressed concrete cross-section is assumed to contain ms reinforcing bars and mp prestressing tendons. Each steel reinforcing bar is identiﬁed by its area, elastic modulus and location with respect to both x- and y-axes, As(i) , Es(i) , xs(i) and ys(i) , respectively. The corresponding properties for the prestressing tendons are Ap(i) , Ep(i) , xp(i) and yp(i) , respectively.

226 Uncracked sections The required geometric properties of the concrete part of the cross-section are its area Ac , its ﬁrst moments of area with respect to both x- and y-axes Bxc and Byc , respectively, the corresponding second moments of area Ixc and Iyc , and the product moment of area Ixyc . Due to the similarities between the derivations proposed in this chapter and those already described in Chapter 5, reference to the latter chapter will be carried out extensively in the following to avoid unnecessary repetition. As in Chapter 5, the proposed procedure is quite general and can be applied with both linear and nonlinear material models, even though in the latter case the integrals of Eq. 6.3 might need to be evaluated numerically.

6.2 Short-term analysis The short-term analysis of a reinforced or prestressed concrete cross-section subjected to axial force and biaxial bending is similar to that already described for uniaxial bending in Chapter 5, with the only addition being that moment equilibrium is enforced with respect to both the x- and y-axes. Based on linear-elastic material properties (Eq. 5.4), the axial equilibrium equation (Eq. 6.2a) can be expressed similarly to Eq. 5.6: Ne,0 = Ni,0 = Nc,0 + Ns,0 + Np,0

(6.5)

As in Chapter 5, the subscript ‘0’ indicates that all variables are calculated at time τ0 before any creep and shrinkage has taken place. In the case of axial force and biaxial bending, Nc,0 , Ns,0 and Np,0 may be expressed in terms of the strain distribution of Eq. 6.1 as: Nc,0 =

σc,0 dA =

Ac

Ec,0 εr,0 + yκx,0 − xκy,0 dA

Ac

= Ac Ec,0 εr,0 + Bxc Ec,0 κx,0 − Byc Ec,0 κy,0 Ns,0 =

ms

(6.6a)

As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0

i=1

= RA,s εr,0 + RBx,s κx,0 − RBy,s κy,0 Np,0 =

(6.6b)

mp Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

mp = RA,p εr,0 + RBx,p κx,0 − RBy,p κy,0 + Ap(i) Ep(i) εp(i),init

(6.6c)

i=1

where RA,s and RA,p represent the axial rigidity of the non-prestressed steel and prestressing tendons, respectively, and RBx,s and RBy,s (RBx,p and RBy,p ) are the ﬁrst moments of the rigidity of the steel reinforcement (prestressing tendons) with respect

Uncracked sections 227 to the x- and y-axes, respectively, and are given by: RA,s =

ms As(i) Es(i)

(6.7a)

i=1 ms RBx,s = ys(i) As(i) Es(i)

(6.7b)

i=1

RBy,s =

ms xs(i) As(i) Es(i)

(6.7c)

i=1 mp RA,p = Ap(i) Ep(i)

(6.7d)

i=1 mp RBx,p = yp(i) Ap(i) Ep(i)

(6.7e)

i=1 mp RBy,p = xp(i) Ap(i) Ep(i)

(6.7f)

i=1

In a similar way, moment equilibrium with respect to the x-axis is enforced using Eq. 6.2b as: Mxe,0 = Mxi,0 = Mxc,0 + Mxs,0 + Mxp,0

(6.8)

in which the internal actions are calculated using: Mxc,0 =

yσc,0 dA =Bxc Ec,0 εr,0 + Ixc Ec,0 κx,0 − Ixyc Ec,0 κy,0

(6.9a)

Ac ms Mxs,0 = ys(i) As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0 i=1

= RBx,s εr,0 + RIx,s κx,0 − RIxy,s κy,0 Mxp,0 =

(6.9b)

mp yp(i) Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

= RBx,p εr,0 + RIx,p κx,0 − RIxy,p κy,0 +

mp yp(i) Ap(i) Ep(i) εp(i),init

(6.9c)

i=1

and RIx,s and RIy,s (RIx,p and RIy,p ) are the rigidities associated with the second moments of area of the steel reinforcement (prestressing tendons) with respect to the

228 Uncracked sections x- and y-axes, respectively, and are given by: ms 2 ys(i) As(i) Es(i) RIx,s =

(6.10a)

i=1

RIxy,s =

ms xs(i) ys(i) As(i) Es(i)

(6.10b)

i=1 mp 2 RIx,p = yp(i) Ap(i) Ep(i)

(6.10c)

i=1 mp RIxy,p = xp(i) yp(i) Ap(i) Ep(i)

(6.10d)

i=1

Finally, considering ﬂexural equilibrium with respect to the y-axis (Eq. 6.2c) gives: Mye,0 = Myi,0 = Myc,0 + Mys,0 + Myp,0 where:

(6.11)

Myc,0 = −

xσc,0 dA = − Byc Ec,0 εr,0 − Ixyc Ec,0 κx,0 + Iyc Ec,0 κy,0

(6.12a)

Ac

Mys,0 = −

ms xs(i) As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0 i=1

= −RBy,s εr,0 − RIxy,s κx,0 + RIy,s κy,0

(6.12b)

mp

Myp,0 = −

xp(i) Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

mp = −RBy,p εr,0 − RIxy,p κx,0 + RIy,p κy,0 − xp(i) Ap(i) Ep(i) εp(i),init

(6.12c)

i=1

and RIy,s =

ms x2s(i) As(i) Es(i)

(6.13a)

i=1 mp RIy,p = x2p(i) Ap(i) Ep(i)

(6.13b)

i=1

Eqs 6.5, 6.8 and 6.11 can be therefore re-written as: mp Ap(i) Ep(i) εp(i),init Ne,0 = RA,0 εr,0 + RBx,0 κx,0 − RBy,0 κy,0 + i=1

(6.14a)

Uncracked sections 229 mp

Mxe,0 = RBx,0 εr,0 + RIx,0 κx,0 − RIxy,0 κy,0 +

yp(i) Ap(i) Ep(i) εp(i),init

(6.14b)

i=1

Mye,0 = −RBy,0 εr,0 − RIxy,0 κx,0 + RIy,0 κy,0 −

mp xp(i) Ap(i) Ep(i) εp(i),init

(6.14c)

i=1

where the cross-sectional rigidities are given by: RA,0 = Ac Ec,0 + RA,s + RA,p

(6.15a)

RIxy,0 = Ixyc Ec,0 + RIxy,s + RIxy,p

(6.15b)

RBx,0 = Bxc Ec,0 + RBx,s + RBx,p

(6.15c)

RBy,0 = Byc Ec,0 + RBy,s + RBy,p

(6.15d)

RIx,0 = Ixc Ec,0 + RIx,s + RIx,p

(6.15e)

RIy,0 = Iyc Ec,0 + RIy,s + RIy,p

(6.15f)

This governing system of equations (Eqs 6.14) can be expressed in compact form as: re,0 = D0 ε0 + fp,init

(6.16)

and using notation similar to that adopted in Chapter 5: ⎡ ⎤ Ne,0 re,0 = ⎣ Mxe,0 ⎦ Mye,0 ⎡ ⎤ RA,0 RBx,0 −RBy,0 D0 = ⎣ RBx,0 RIx,0 −RIxy,0 ⎦ −RBy,0 −RIxy,0 RIy,0 ⎡ ⎤ εr,0 ε0 = ⎣ κx,0 ⎦ κy,0 ⎡ ⎤ mp Ap(i) Ep(i) ⎣ yp(i) Ap(i) Ep(i) ⎦ εp(i),init fp,init = i=1 −xp(i) Ap(i) Ep(i)

(6.17a)

(6.17b)

(6.17c)

(6.17d)

The unknown strain vector ε0 is obtained by solving Eq. 6.16 and is given by: re,0 − fp,init = F0 re,0 − fp,init (6.18) ε0 = D−1 0 in which ⎡ RIx,0 RIy,0 −R2Ixy,0 1 ⎢ F0 = ⎣RBy,0 RIxy,0 −RBx,0 RIy,0 R0 RBy,0 RIx,0 −RBx,0 RIxy,0

RBy,0 RIxy,0 −RBx,0 RIy,0 RA,0 RIy,0 −R2By,0 RA,0 RIxy,0 −RBx,0 RBy,0

⎤ RBy,0 RIx,0 −RBx,0 RIxy,0 ⎥ RA,0 RIxy,0 −RBx,0 RBy,0 ⎦ 2 RA,0 RIx,0 −RBx,0 (6.19a)

230 Uncracked sections and R0 = RA,0 RIx,0 RIy,0 − R2Ixy,0 − R2Bx,0 RIy,0 + 2RBx,0 RBy,0 RIxy,0 − R2By,0 RIx,0 (6.19b) The strain at any point (x, y) is obtained by substituting Eq. 6.18 into Eq. 6.1: ε0 = εr,0 + yκx,0 − xκy,0 = 1 y −x ε0

(6.20)

and the stress at any point can then be determined from the calculated strain (Eq. 6.20) using the appropriate constitutive relationship (Eqs 5.4). By setting Eq. 6.20 equal to zero, the equation of the line (in the x-y plane) deﬁning the neutral axis may be expressed as y=

κy,0 εr,0 x− κx,0 κx,0

(6.21)

Equation 6.21 is not deﬁned when κx,0 = 0, in which case the problem degenerates to one of axial force and uniaxial bending about the y-axis and can be solved using the methods of Chapter 5. The slope of the neutral axis at time τ0 may be obtained by differentiating Eq. 6.21 and (adopting clockwise rotations to be positive similarly to θM,0 ) is expressed as a function of the applied moments and ﬂexural rigidities: tan θNA,0 =

κy,0 κx,0

(6.22)

The neutral axis (Eq. 6.21) intersects the y-axis at: y(x = 0) = −

εr,0 κx,0

(6.23)

If the cross-section is doubly-symmetric (as is often the case in practice), the expression for F0 can be simpliﬁed by placing the origin of the coordinate system at the centroid of the cross-section and specifying the orthogonal axes to be parallel to the axes of symmetry (leading to RIxy,0 = RBx,0 = RBy,0 = 0). Therefore: ⎡

RIx,0 RIy,0 ⎣ 0 F0 = RA,0 RIx,0 RIy,0 0 1

0 RA,0 RIy,0 0

⎤ 0 ⎦ 0 RA,0 RIx,0

(6.24)

Without prestressing (usually the case for columns), using Eq. 6.24 in Eq. 6.18, the expression for the strain at a point ε0 simpliﬁes to: ε0 = εr,0 + yκx,0 − xκy,0 =

Mye,0 Ne,0 Mxe,0 +y −x RA,0 RIx,0 RIy,0

(6.25)

Uncracked sections 231 In this particular case (i.e. no prestressing), the equation of the line (in the x-y plane) deﬁning the neutral axis may be expressed in terms of external loads as: y=

RIx,0 Ne,0 RIx,0 Mye,0 x− RIy,0 Mxe,0 RA,0 Mxe,0

(6.26)

with corresponding slope and intersect with the y-axis calculated using: tan θNA,0 =

RIx,0 Mye,0 RIx,0 = tan θM,0 RIy,0 Mxe,0 RIy,0

(6.27a)

and y(x = 0) = −

RIx,0 Ne,0 RA,0 Mxe,0

(6.27b)

Evidently, the angle of the applied moment Me,0 (i.e. θM,0 ) and of the neutral axis (i.e. θNA,0 ) coincide only when the ﬂexural rigidities calculated with respect to both the x- and y-axes are identical, i.e. when RIx,0 = RIy,0 (Eq. 6.27a). In all other cases, these two angles differ from each other (Fig. 6.2). Moreover, the angle of the neutral axis θNA,0 may vary with time, as will be seen subsequently. The cross-sectional rigidities could have also been calculated from the transformed section, where the areas of the reinforcing bars and bonded prestressing tendons (As(i) and Ap(i) , respectively) are transformed into equivalent areas of concrete (ns(i),0 As(i) and np(i),0 Ap(i) , respectively), where ns(i),0 = Es(i) /Ec,0 is the modular ratio of the i-th steel bar and np(i),0 = Ep(i) /Ec,0 is the modular ratio of the i-th tendon. In this case, the cross-sectional rigidities are given by: RA,0 = A0 Ec,0

(6.28a)

RBx,0 = Bx,0 Ec,0

(6.28b)

RBy,0 = By,0 Ec,0

(6.28c)

RIx,0 = Ix,0 Ec,0

(6.28d)

RIy,0 = Iy,0 Ec,0

(6.28e)

RIxy,0 = Ixy,0 Ec,0

(6.28f)

x

Mxe,0

x

qM,0

qNA,0 er,0

y Mye,0 (a) Orientation of Me

Neutral axis

Me,0 y

(b) Orientation of the neutral axis

Figure 6.2 Orientations of applied moments and neutral axis.

k0

e

232 Uncracked sections where A0 is the area of the transformed concrete section; Bx,0 and Ix,0 are the transformed ﬁrst and second moments of area calculated with respect to the x-axis, respectively; By,0 and Iy,0 represent the corresponding moments of area with respect to the y-axis; and Ixy,0 is the product moment of area. Using Eqs 6.28, the matrix F0 , previously introduced in Eq. 6.19a, can be expressed as: ⎡

2 Ix,0 Iy,0 −Ixy,0 1 ⎢ F0 = ⎣ By,0 Ixy,0 −Bx,0 Iy,0 S0 Ec,0 By,0 Ix,0 −Bx,0 Ixy,0

By,0 Ixy,0 −Bx,0 Iy,0 A0 Iy,0 −B2y,0 A0 Ixy,0 −Bx,0 By,0

⎤ By,0 Ix,0 −Bx,0 Ixy,0 ⎥ A0 Ixy,0 −Bx,0 By,0 ⎦ A0 Ix,0 −B2x,0 (6.29a)

and 2 − B2x,0 Iy,0 + 2Bx,0 By,0 Ixy,0 − B2y,0 Ix,0 S0 = A0 Ix,0 Iy,0 − Ixy,0

(6.29b)

Considering the particular case of a doubly-symmetric section with the origin at the centroid of the section and orthogonal axes parallel to the axes of symmetry (for which RIxy,0 = RBx,0 = RBy,0 = 0), F0 simpliﬁes to: ⎡ Ix,0 Iy,0 1 ⎣ 0 F0 = A0 Ix,0 Iy,0 Ec,0 0

0 A0 Iy,0 0

⎤ 0 ⎦ 0 A0 Ix,0

(6.30)

Without prestressing effects, the strain at any point (x, y) can be calculated using: ε0 = εr,0 + yκx,0 − xκy,0 =

Mye,0 Ne,0 Mxe,0 +y −x A0 Ec,0 Ix,0 Ec,0 Iy,0 Ec,0

(6.31)

By setting ε0 = 0 in Eq. 6.31, the equation of the neutral axis, its slope and its intersection with the y-axis are obtained as functions of the transformed second moments of area and are given by: y= tan θNA,0 =

Ix,0 Ne,0 Ix,0 Mye,0 x− Iy,0 Mxe,0 A0 Mxe,0

(6.32a)

Ix,0 tan θM,0 Iy,0

(6.32b)

Ix,0 Ne,0 A0 Mxe,0

(6.32c)

y(x = 0) = −

As discussed in Chapter 5, the calculation of the cross-sectional rigidities based on the transformed section using Eqs 6.28 is equivalent to calculation using Eqs 6.15. Either approach can be used depending on the preference of the structural designer.

Uncracked sections 233

Example 6.1 The doubly-symmetric reinforced concrete cross-section shown in Fig. 6.3 is subjected to biaxial bending, with Mxe = 5 kNm and Mye = 10 kNm. In this example, the axial force is zero (i.e. Ne,0 = 0 kN). The stress and strain distributions are to be determined at time τ0 , assuming the origin of the coordinate system is located at the centroid of the cross-section and the x- and y-axes are parallel to the axes of symmetry (i.e. dx.ref = b/2 and dy.ref = D/2 measured from the left and top of the section, respectively, as shown in Fig. 6.3). Both concrete and reinforcement are assumed to be linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = ns(j),0 = Es /Ec,0 = 6.25 (with j = 1, . . ., 4). b = 300 dx.ref = 150 As(1) = 450 mm2

150

90

90 As(2) = 450 mm2

dy.ref = 150 90

x

D = 300

As(3) = 450 mm2

90 150

As(4) = 450 mm2

y

Figure 6.3 Reinforced concrete cross-section for Example 6.1 (dimensions in mm).

Based on the adopted reference system the coordinates of each of the four steel reinforcing bars are: xs(1) = −90 mm ys(1) = −90 mm xs(2) = 90 mm ys(2) = −90 mm xs(3) = 90 mm ys(3) = 90 mm xs(4) = −90 mm ys(4) = 90 mm For this reinforced concrete section, the vectors re,0 and f p,init are ⎤ ⎡ ⎡ ⎤ 0N 0N re,0 = ⎣ 5 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 10 × 106 Nmm

234 Uncracked sections Based on the transformed section, the relevant cross-sectional properties are calculated as: A0 = bD+(ns,0 −1)[As(1) +As(2) +As(3) +As(4) ] = 300×300+(6.25−1)×(4×450) = 99,450 mm2 ;

2 bD3 D 2 2 2 Ix,0 = +As(2) ys(2) +As(3) ys(3) +bD −dy.ref +(ns,0 −1) As(1) ys(1) 12 2 300×3003 2 +As(4) ys(4) = +3002 (150−150)2 12 +5.25×[2×450×(−90)2 +2×450×902 ] = 751.5×106 mm4 . From the double symmetry and the adopted coordinate system: Iy,0 = Ix,0 = 751.5 × 106 mm4 and Bx,0 = By,0 = Ixy,0 = 0. From Eq. 6.30: ⎡ ⎤ Ix,0 Iy,0 0 0 1 ⎢ ⎥ F0 = 0 A0 Iy,0 0 ⎣ ⎦ A0 Ix,0 Iy,0 Ec,0 0 0 A0 Ix,0 1 99,450×(751.5×106 ) 2 × 32,000 ⎤ ⎡ 2 6 751.5×10 0 0 ⎥ ⎢ ⎥ ×⎢ 0 99,450×751.5×106 0 ⎦ ⎣ 0 0 99,450×751.5×106 ⎤ ⎡ 3.142×10−10 N−1 0 0 ⎥ ⎢ =⎣ 0 4.158×10−14 N−1 mm−2 0 ⎦ 0 0 4.158×10−14 N−1 mm−2 =

The strain ε0 is then determined based on Eq. 6.18: ⎤ ⎡ 3.142 × 10−10 0 0 ⎦ ε0 = F0 re,0 − fp,init = ⎣ 0 4.158 × 10−14 0 0 0 4.158 × 10−14 ⎧⎡ ⎤ ⎡ ⎤⎫ 0 0 ⎬ ⎨ × ⎣ 5 × 106 ⎦ − ⎣ 0 ⎦ ⎭ ⎩ 0 10 × 106 ⎤ ⎡ 0 = ⎣ 0.208 × 10−6 mm−1 ⎦ 0.416 × 10−6 mm−1

Uncracked sections 235 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = 0 κx,0 = 0.208 × 10−6 mm−1 κy,0 = 0.416 × 10−6 mm−1 and, from Eq. 6.1, the strains at the corners of the cross-section become: ε0 (x = −b/2, y = −D/2) = (0 − 150 × 0.208 − (−150) × 0.416) × 10−6 = 31.2 × 10−6 ε0 (x = b/2, y = −D/2) = (0 − 150 × 0.208 − 150 × 0.416) × 10−6 = −93.6 × 10−6 ε0 (x = b/2, y = D/2) = (0 + 150 × 0.208 − 150 × 0.416) × 10−6 = −31.2 × 10−6 ε0 (x = −b/2, y = D/2) = (0 + 150 × 0.208 − (−150) × 0.416) × 10−6 = 93.6 × 10−6 The stresses in the concrete at the four corners of the cross-section are obtained from Eq. 5.16a: σc,0(top-left) = Ec,0 ε0(top-left) = 32 × 103 × 31.2 × 10−6 = 1.00 MPa σc,0(top-right) = −2.99 MPa σc,0(btm-right) = −1.00 MPa σc,0(btm-left) = 2.99 MPa Similarly, the stress in each reinforcement bar is calculated using Eq. 5.16b: σs(1),0 = Es 1 ys(1) −xs(1) ε0 ⎡ ⎤ 0 = 200 × 103 × [1 − 90 − (−90)] × ⎣ 0.208 × 10−6 ⎦ 0.416 × 10−6 = 3.7 MPa; σs(2),0 = −11.2 MPa σs(3),0 = −3.7 MPa σs(4),0 = 11.2 MPa The slopes of both applied moment Me and of the neutral axis are calculated as (Eqs 6.4 and 6.32b): tan θM,0 = tan θNA,0 =

Mye,0 10 × 106 = = 2.0 from which θM,0 = 63.43◦ and Mxe,0 5 × 106 Ix,0 751.5 × 106 tan θM,0 = × 2.0 = 2.0 Iy,0 751.5 × 106 and therefore θNA,0 = 63.43◦ .

As expected, θM,0 = θNA,0 because Ix,0 = Iy,0 .

236 Uncracked sections The strain and stress distributions are plotted in Fig. 6.4. The cross-sectional rigidities could have also been calculated based on Eqs 6.15: RA,0 = 3182 × 106 N RIx,0 = RIy,0 = 24.05 × 1012 Nmm2 RBx,0 = RBy,0 = RIxy,0 = 0 In this case, F0 is obtained from Eq. 6.24 and is identical to that calculated above.

x 63.43°

Neutral axis

−93.6 × 10−6

y

−2.99

e −11.2

93.6 × 10−6 −3.7 3.7 2.99

s

11.2

Figure 6.4 Initial strain and stress diagrams at time τ0 for Example 6.1 (all units in mm, MPa).

Example 6.2 The strain and stress distributions on the reinforced concrete cross-section shown in Fig. 6.5 are to be determined at time τ0 when the applied actions, Ne = −500 kN (compression), Mxe = 25 kNm and Mye = 25 kNm, are ﬁrst applied. The origin of the coordinate system is taken at the centroid of the section and the x- and y-axes are assumed to be parallel to the axes of symmetry (i.e. dx.ref = b/2 and dy.ref = D/2 measured from the left and top of the section, respectively).

Uncracked sections 237 The material behaviour is linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for all reinforcement is therefore ns,0 = Es /Ec,0 = 6.25. b = 300 dx.ref = 150

As(j) = 450 mm2

150

90

for j = 1,…,6

90

As(2)

As(1)

dy.ref = 200 150 x D = 400

As(4)

As(3)

150 200 As(5)

As(6) y

Figure 6.5 Reinforced concrete cross-section for Example 6.2 (dimensions in mm).

Based on the adopted reference system, the coordinates of the steel reinforcement are: xs(1) = −90 mm ys(1) = −150 mm xs(2) = 90 mm ys(2) = −150 mm xs(3) = −90 mm ys(3) = 0 mm xs(4) = 90 mm ys(4) = 0 mm xs(5) = −90 mm ys(5) = 150 mm xs(6) = 90 mm ys(6) = 150 mm The vectors of external loads and prestressing are: ⎡ ⎡ ⎤ ⎤ −500 × 103 N 0N re,0 = ⎣ 25 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 25 × 106 Nmm The properties of the transformed cross-section are: A0 = bD + (ns,0 − 1)

6 0 i=1

As(i) = 134.1 × 103 mm2

238 Uncracked sections

2 6 0 bD3 D 2 = 1812 × 106 mm4 Ix,0 = + bD − dy.ref + (ns,0 − 1) As(i) ys(i) 12 2 i=1

2 6 0 Db3 b Iy,0 = + bD − dx.ref + (ns,0 − 1) As(i) x2s(i) = 1014 × 106 mm4 12 2 i=1 For this cross-section and for these coordinate axes: Bx,0 = By,0 = Ixy,0 = 0. From Eq. 6.30: ⎡

⎤ 2.329×10−10 N−1 0 0 ⎢ ⎥ F0 = ⎣ 0 1.724×10−14 N−1 mm−2 0 ⎦ 0 0 3.080×10−14 N−1 mm−2

and ε0 is calculated using Eq. 6.18: ⎡ ⎤ −116.4 × 10−6 ε0 = F0 re,0 − fp,init = ⎣ 0.431 × 10−6 mm−1 ⎦ 0.770 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = −116.4 × 10−6 κx,0 = 0.431 × 10−6 mm−1 κy,0 = 0.770 × 10−6 mm−1 . The strains at the four corners of the cross-section are (Eq. 6.1): ε0(top-left) (x = −b/2, y = −D/2) = −87.2 × 10−6 ε0(top-right) (x = b/2, y = −D/2) = −318.1 × 10−6 ε0(btm-right) (x = b/2, y = D/2) = −145.7 × 10−6 ε0(btm-left) (x = −b/2, y = D/2) = 85.2 × 10−6 and the concrete and steel stress distributions are calculated using Eq. 5.16: σc,0(top-left) = Ec,0 ε0(top-left) = −2.79 MPa σc,0(top-right) = −10.18 MPa σc,0(btm-right) = −4.66 MPa σc,0(btm-left) = 2.73 MPa σs(1),0 = Es 1 ys(1) −xs(1) ε0 ⎡ ⎤ −116.4 × 10−6 = 200 × 103 × [1 − 150 − (−90)] × ⎣ 0.431 × 10−6 ⎦ 0.770 × 10−6 = −22.4 MPa; σs(2),0 = −50.1 MPa

Uncracked sections 239 σs(3),0 = −9.4 MPa σs(4),0 = −37.1 MPa σs(5),0 = 3.50 MPa σs(6),0 = −24.2 MPa The slopes of both applied moment Me,0 and of the neutral axis are (Eqs 6.4 and 6.32b): tan θM,0 =

tan θNA,0 =

Mye,0 25 × 106 = = 1.0 and therefore θM,0 = 45◦ and Mxe,0 25 × 106 Ix,0 1812 × 106 tan θM = × 1 = 1.79 Iy,0 1014 × 106 and therefore θNA,0 = 60.76◦ .

The calculated stresses and strains are shown in Fig. 6.6.

60.76°

x

Neutral axis

45° Me,0

−318.1 × 10−6

y

−10.18 e

85.2 × 10−6

−9.4

−37.1 −24.2 −22.4

−50.1

3.5 2.73

s

Figure 6.6 Initial strain and stress diagrams at time τ0 for Example 6.2 (all units in mm, MPa).

240 Uncracked sections In this case θM,0 = θNA,0 (since Ix,0 = Iy,0 ), and the neutral axis passes through the y-axis at (Eq. 6.32c): y=−

1812 × 106 −500 × 103 Ix,0 Ne,0 =− = 270.2 mm A0 Mxe,0 134.1 × 103 25 × 106

The cross-sectional rigidities could have also been calculated based on Eqs 6.15: RA,0 = 4293 × 106 N RIx,0 = 58 × 1012 Nmm2 RIy,0 = 32.47 × 1012 Nmm2 RBx,0 = RBy,0 = RIxy,0 = 0 In this case, F0 is obtained from Eq. 6.24 and is identical to that calculated above.

Example 6.3 For the reinforced concrete cross-section shown in Fig. 6.7, the strain and stress distributions are to be calculated at time τ0 . The section is subjected to: Ne = −800 kN (compression), Mxe = 50 kNm and Mye = 25 kNm. The origin b = 480

As(j) = 450 mm2 for j = 1, .. ,8

dx.ref = 215.6

1

60

180

180

60

2 60

As(2)

As(1)

As(3) D1 = 300

dy.ref = 215.6

180 x D = 480 As(4)

As(5)

As(6)

4

b2 = 180

3

60

120 D2 = 180

As(7)

As(8)

6

60

5 b1 = 300 y

Figure 6.7 Reinforced concrete cross-section for Example 6.3 (dimensions in mm).

Uncracked sections 241 of the coordinate system is taken at the centroid of the section (calculated based on instantaneous material properties) located at dx.ref = dy.ref = 215.6 mm, as shown in Fig. 6.7. The material behaviour is linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for all reinforcement is therefore ns,0 = Es /Ec,0 = 6.25. Based on the adopted reference system, the coordinates of the steel reinforcement are: xs(1) = −155.6 mm; ys(1) = −155.6 mm xs(2) = 24.4 mm; ys(2) = −155.6 mm xs(3) = 204.4 mm; ys(3) = −155.6 mm xs(4) = −155.6 mm; ys(4) = 24.4 mm xs(5) = 24.4 mm; ys(5) = 24.4 mm xs(6) = 204.4 mm; ys(6) = 24.4 mm xs(7) = −155.6 mm; ys(7) = 204.4 mm xs(8) = 24.4 mm; ys(8) = 204.4 mm and the coordinates of the corners of the concrete section (numbered 1–6 in Fig. 6.7) are: x(1) = −215.6 mm; y(1) = −215.6 mm x(2) = 264.4 mm; y(2) = −215.6 mm x(3) = 264.4 mm; y(3) = 84.4 mm xs(4) = 84.4 mm; ys(4) = 84.4 mm xs(5) = 84.4 mm; ys(5) = 264.4 mm xs(6) = −215.6 mm; ys(6) = 264.4 mm The vectors of external loads and prestressing are: ⎡ ⎡ ⎤ ⎤ −800 × 103 N 0N re,0 = ⎣ 50 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 25 × 106 Nmm The properties of the transformed cross-section are: 8 0 A0 = bD − b2 D2 + (ns,0 − 1) As(i) = 216.9 × 103 mm2

i=1

D1 D2 Bx,0 = bD1 − dy.ref + b1 D2 D1 + − dy.ref 2 2 8 0 As(i) ys(i) = 0 mm3 + (ns,0 − 1) i=1

8 0 b b1 By,0 = bD1 − dx.ref + b1 D2 − dx.ref + (ns,0 − 1) As(i) xs(i) 2 2 i=1 = 0 mm3

2

2 bD31 b1 D32 D1 D2 Ix,0 = + bD1 + + b 1 D2 D 1 + + − dy.ref − dy.ref 12 12 2 2 8 0 2 = 3861 × 106 mm4 (ns,0 − 1) As(i) ys(i) i=1

242 Uncracked sections Iy,0 =

2

2 D2 b31 D1 b3 b b1 + bD1 − dx.ref + + b1 D2 − dx.ref 12 2 12 2 8 0 + (ns,0 − 1) As(i) x2s(i) = 3861 × 106 mm4 ; i=1

D1 b D2 Ixy,0 = bD1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref + (ns,0 − 1) As(i) xs(i) ys(i) = −934.3 × 106 mm4 . × 2 i=1 The fact that Bx,0 = By,0 = 0 could have also been concluded by noting that the origin of the coordinate system coincides with the centroid of the cross-section. Considering the ﬁrst moments of area about both axes are nil (i.e. Bx,0 = By,0 = 0), Eq. 6.29a simpliﬁes to: ⎡

⎤ 2 Ix,0 Iy,0 − Ixy,0 0 0 ⎣ F0 = 0 A0 Iy,0 A0 Ixy,0 ⎦ 2 A0 Ix,0 Iy,0 − Ixy,0 Ec,0 0 A0 Ixy,0 A0 Ix,0 1

⎡

⎤ 1.441 × 10−10 0 0 =⎣ 0 8.597 × 10−15 −2.080 × 10−15 ⎦ 0 −2.080 × 10−15 8.597 × 10−15 and ε0 is calculated using Eq. 6.18: ⎤ ⎡ −115.3 × 10−6 ε0 = F0 re,0 − fp,init = ⎣ 0.378 × 10−6 mm−1 ⎦ 0.111 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = −115.3 × 10−6 κx,0 = 0.378 × 10−6 mm−1 κy,0 = 0.111 × 10−6 mm−1 The strains at the corners of the cross-section are obtained from Eq. 6.1: ε0(corner 1) = −172.8 × 10−6 ε0(corner 2) = −226.0 × 10−6 ε0(corner 3) = −112.6 × 10−6 ε0(corner 4) = −92.7 × 10−6 ε0(corner 5) = −24.6 × 10−6 ε0(corner 6) = 8.55 × 10−6

Uncracked sections 243 and the corresponding concrete stresses are obtained using Eq. 5.16a: σc,0(corner 1) = Ec,0 ε0(corner 1) = −5.53 MPa σc,0(corner 2) = −7.23 MPa σc,0(corner 3) = −3.60 MPa σc,0(corner 4) = −2.97 MPa σc,0(corner 5) = −0.79 MPa σc,0(corner 6) = 0.27 MPa The strains in the steel reinforcing bars are: εs(1),0 = −156.8 × 10−6 εs(2),0 = −176.8 × 10−6 εs(3),0 = −196.7 × 10−6 εs(4),0 = −88.8 × 10−6 εs(5),0 = −108.7 × 10−6 εs(6),0 = −128.7 × 10−6 εs(7),0 = −20.8 × 10−6 εs(8),0 = −40.7 × 10−6 and from Eq. 5.16b, the steel stresses are: σs(1),0 = −31.4 MPa σs(2),0 = −35.4 MPa σs(3),0 = −39.3 MPa σs(4),0 = −17.8 MPa σs(5),0 = −21.7 MPa σs(6),0 = −25.7 MPa σs(7),0 = −4.15 MPa σs(8),0 = −8.14 MPa The slope of the applied moment Me,0 is calculated based on Eq. 6.4: tan θM,0 =

Mye,0 25 × 106 = = 0.5 and therefore θM,0 = 26.56◦ Mxe,0 50 × 106

while the slope of the neutral axis is obtained using Eq. 6.22: tan θNA,0 =

κy,0 0.111 × 10−6 = = 0.293 and therefore θNA,0 = 16.31◦ . κx,0 0.378 × 10−6

The intersection of the neutral axis with the y-axis is calculated from Eq. 6.23: y(x = 0) = −

εr,0 −115.3 × 10−6 =− = +304.8 mm. κx,0 0.378 × 10−6

244 Uncracked sections The calculated stresses and strains are shown in Fig. 6.8. 16.31° −226.0 × 10−6 −7.23 x

−39.3 −35.4 −31.4

Me,0

−25.7 −21.7 Neutral axis

−17.8 y −8.14

e 8.55 × 10−6

−4.15 0.27

s

Figure 6.8 Initial strain and stress diagrams at time τ0 for Example 6.3 (all units in mm, MPa).

6.3 Long-term analysis using the age-adjusted effective modulus method (AEMM) The time analysis based on the AEMM to determine stresses and strains on a crosssection at time τk after a period of sustained loading was presented in Chapters 4 and 5 and only the steps relevant to the case of biaxial bending will be presented here. The constitutive relationships adopted for the concrete and steel are those already deﬁned for the AEMM in Eqs 5.22. With the instantaneous stress and strain distributions determined at time τ0 using the analysis of the previous section, the strain diagram at time τk is deﬁned by the strain at the origin and the curvatures about the orthogonal reference axes, i.e. εr,k , κx,k and κy,k . These are obtained by solving the equilibrium equations deﬁned by: re,k = ri,k

(6.33)

where T re,k = Ne,k Mxe,k Mye,k

(6.34a)

Uncracked sections 245 and T ri,k = Ni,k Mxi,k Myi,k

(6.34b)

Based on the material constitutive relationships (Eqs 5.22), the axial force resisted by each component of the cross-section at τk can be determined from: Nc,k = σc,k dA = Ee,k εr,k + yκx,k − xκy,k − εsh,k + Fe,0 σc,0 dA Ac

Ac

= Ac Ee,k εr,k + Bxc Ee,k κx,k − Byc Ee,k κy,k − Ac Ee,k εsh,k + Fe,0 Nc,0 Ns,k = RA,s εr,k + RBx,s κx,k − RBy,s κy,k Np,k = RA,p εr,k + RBx,p κx,k − RBy,p κy,k +

(6.35a) (6.35b)

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

(6.35c) These expressions can be summed to give the axial force resisted by the whole section Ni,k : Ni,k = RA,k εr,k + RBx,k κx,k − RBy,k κy,k − Ac Ee,k εsh,k + Fe,0 Nc,0 +

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36a)

i=1

and, in a similar manner, the internal moments about the x- and y-axes can be determined from: Mxi,k = RBx,k εr,k + RIx,k κx,k − RIxy,k κy,k − Bxc Ee,k εsh,k + Fe,0 Mxc,0 +

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36b)

i=1

Myi,k = −RBy,k εr,k − RIxy,k κx,k + RIy,k κy,k + Byc Ee,k εsh,k + Fe,0 Myc,0 −

mp

xp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36c)

i=1

where the time-dependent cross-sectional rigidities at time τk are determined from expressions similar to those at time τ0 (Eqs 6.15) except that the age-adjusted effective modulus of the concrete Ee,k is used instead of the elastic modulus Ec,0 . That is: RA,k = Ac Ee,k + RA,s + RA,p

(6.37a)

RIxy,k = Ixyc Ee,k + RIxy,s + RIxy,p

(6.37b)

RBx,k = Bxc Ee,k + RBx,s + RBx,p

(6.37c)

246 Uncracked sections RBy,k = Byc Ee,k + RBy,s + RBy,p

(6.37d)

RIx,k = Ixc Ee,k + RIx,s + RIx,p

(6.37e)

RIy,k = Iyc Ee,k + RIy,s + RIy,p

(6.37f)

Substituting Eqs 6.36 into Eq. 6.33 produces the equilibrium equations describing the structural response at τk : re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k where

⎤ εr,k εk = ⎣ κx,k ⎦ κy,k ⎡ ⎤ RA,k RBx,k −RBy,k Dk = ⎣ RBx,k RIx,k −RIxy,k ⎦ −RBy,k −RIxy,k RIy,k ⎡ ⎤ ⎡ ⎤ Ac εr,0 + Bxc κx,0 − Byc κy,0 Nc,0 ⎢ ⎥ fcr,k = Fe,0 ⎣ Mxc,0 ⎦ = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ Myc,0 −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 ⎤ ⎡ Ac ⎥ ⎢ fsh,k = ⎣ Bxc ⎦ Ee,k εsh,k −Byc

(6.38)

⎡

(6.39a)

(6.39b)

(6.39c)

(6.39d)

The variables describing the strain diagram at τ0 , i.e. εr,0 , κx,0 and κy,0 , are assumed to be known from the instantaneous analysis. The initial prestressing is included in f p,init (already deﬁned for the instantaneous analysis in Eq. 6.17d) and the steel relaxation is considered by means of f p.rel,k calculated as: ⎡ ⎤ mp A E p(i) p(i) ⎢ ⎥ (6.40) fp.rel,k = ⎣ yp(i) Ap(i) Ep(i) ⎦ εp(i),init ϕp (τk , σp(i),init ) i=1 −xp(i) Ap(i) Ep(i) Solving Eq. 6.38, the strain diagram at time τk is given by: εk = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(6.41)

where ⎡

⎤ RBy,k RIxy,k −RBx,k RIy,k RBy,k RIx,k −RBx,k RIxy,k RIx,k RIy,k −R2Ixy,k 1 ⎢ RA,k RIy,k −R2By,k RA,k RIxy,k −RBx,k RBy,k ⎥ Fk = ⎣ RBy,k RIxy,k −RBx,k RIy,k ⎦ Rk RBy,k RIx,k −RBx,k RIxy,k RA,k RIxy,k −RBx,k RBy,k RA,k RIx,k −R2Bx,k

(6.42a)

Uncracked sections 247 and Rk = RA,k RIx,k RIy,k − R2Ixy,k − R2Bx,k RIy,k + 2RBx,k RBy,k RIxy,k − R2By,k RIx,k (6.42b) The stress distribution at time τk can then be calculated using equations similar to Eqs 5.41 as follows: & ' Ee,k εk − εsh,k + Fe,0 σc,0 = Fe,0 σc,0 Ee,k 1 y −x εk − εsh,k + σc,k = (6.43a) σs,k(i) = Es(i) εk = Es(i) 1 ys(i) − xs(i) εk (6.43b) σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) − xp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(6.43c)

where at any point (x, y) on the cross-section εk = εr,k + yκx,k − xκy,k = 1 y −x εk . Similar to Eq. 6.21, the position of the neutral axis at time τk is given by: y=

κy,k κx,k

x−

εr,k κx,k

(6.44)

while its slope and its intersect with the y-axis may be calculated using: tan θNA,k =

κy,k

(6.45a)

κx,k εr,k y(x = 0) = − κx,k

(6.45b)

The expression for Fk can be signiﬁcantly simpliﬁed for doubly symmetric crosssections when the origin is located at the centroid of the section and the orthogonal axes are parallel to the axes of symmetry. In this case, RIxy,k = RBx,k = RBy,k = 0 and Fk is given by: ⎡

⎤ RIx,k RIy,k 0 0 1 ⎢ ⎥ 0 RA,k RIy,k 0 Fk = ⎣ ⎦ RA,k RIx,k RIy,k 0 0 RA,k RIx,k

(6.46)

As discussed previously for the instantaneous analysis, the cross-sectional rigidities included in Fk can be calculated based on the properties of the age-adjusted transformed cross-section. For this purpose, modular ratios of n¯ s(i),k = Es(i) / Ee,k and n¯ p(i),k = Ep(i) / Ee,k are to be used for the i-th steel bar and the i-th tendon, respectively.

248 Uncracked sections

Example 6.4 For the reinforced concrete section and coordinate system of Example 6.2 (Fig. 6.5), if the external actions (i.e. Ne = −500 kN, Mxe = 25 kNm, Mye = 25 kNm) are sustained over a period of time (τ0 to τk ), the longterm effects caused by creep and shrinkage are to be determined. As for Example 6.2, Ec,0 = 32 GPa, Es = 200 GPa, and ns,0 = Es /Ec,0 = 6.25. The creep coefﬁcient, the ageing coefﬁcient and the shrinkage strain associated with the time period under consideration are ϕ(τk , τ0 ) = 2.0; χ(τk , τ0 ) = 0.65 and εsh (τk ) = −400 × 10−6 . From Example 6.2 at τ0 : εr,0 = −116.4 × 10−6 ; κx0 = 0.431 × 10−6 mm−1 ; κy0 = 0.770 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 32,000 = 13,910 MPa = 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.0 and therefore n¯ s,k = 14.38

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.0 × (0.65 − 1.0) Fe,0 = = −0.304 = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.0 For this reinforced concrete section, the vectors re,k , fp,init and fp.rel,k in Eq. 6.41 are: ⎡ ⎤ −500 × 103 N ⎢ ⎥ re,k = ⎣ 25 × 106 Nmm ⎦ 25 × 106 Nmm ⎡ ⎤ 0N ⎢ ⎥ fp,init = ⎣ 0 Nmm ⎦ 0 Nmm ⎡ ⎤ 0N ⎢ ⎥ fp.rel,k = ⎣ 0 Nmm ⎦ 0 Nmm The properties of the age-adjusted transformed cross-section based on Ee,k are: 6 0 ¯ k = bD + (n¯ s,k − 1) As(i) = 156.1 × 103 mm2 A

2 i=1 3 6 0 bD D 2 = 2141 × 106 mm4 I¯x,k = + bD − dy.ref + (n¯ s,k − 1) As(i) ys(i) 12 2 i=1

2 6 0 Db3 b I¯y,k = + bD − dx.ref + (n¯ s,k − 1) As(i) x2s(i) = 1192 × 106 mm4 12 2 i=1 B¯ x,k = B¯ y,k = I¯xy,k = 0

Uncracked sections 249 The geometric properties of the concrete are required for the calculation of f cr,k and f sh,k and are obtained as follows: Ac = bD −

6 0

As(i) = 117.3 × 103 mm2

2 6 0 bD3 D 2 = 1559 × 106 mm4 Ixc = + bD − dy.ref − As(i) ys(i) 12 2 i=1

2 6 0 Db3 b Iyc = + bD As(i) x2s(i) = 878.1 × 106 mm4 − dx.ref − 12 2 i=1 Bxc = Byc = Ixyc = 0 i=1

From Eqs 6.39c and d: ⎡

⎤ ⎡ ⎤ 133.0 × 103 N Ac εr,0 + Bxc κx,0 − Byc κy,0 fcr,k = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ = ⎣ −6.55 × 106 Nmm ⎦ −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 −6.58 × 106 Nmm ⎤ ⎤ ⎡ ⎡ 117.3 × 103 −652.8 × 103 N −6 ⎦ ⎦ × 13,910 × −400 × 10 =⎣ fsh,k = ⎣ 0 Nmm 0 0 Nmm 0 Based on properties of the age-adjusted transformed cross-section, Fk is calculated using Eq. 6.46 as: ⎡

⎤ 4.604×10−10 N−1 0 0 ⎢ ⎥ Fk = ⎣ 0 3.356×10−14 N−1 mm−2 0 ⎦ −1 −14 −2 0 0 6.027 ×10 N mm

The strain εk at time τk is obtained using Eq. 6.41: ⎤ ⎡ −592.0 × 10−6 εk = Fk (re,k − fcr,k + fsh,k ) = ⎣ 1.058 × 10−6 mm−1 ⎦ 1.903 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,k = −592.0 × 10−6 κx,k = 1.058 × 10−6 mm−1 κy,k = 1.903 × 10−6 mm−1 The strains at the corners of the cross-section are (Eq. 6.1): εk(top-left) (x = −b/2, y = −D/2) = −518.2 × 10−6 εk(top-right) (x = b/2, y = −D/2) = −1089 × 10−6 εk(btm-right) (x = b/2, y = D/2) = −665.8 × 10−6 εk(btm-left) (x = −b/2, y = D/2) = −94.7 × 10−6

250 Uncracked sections The stresses in the concrete and in the steel reinforcement are calculated using Eqs 5.16: & ' σc,k(top-left) = Fe,0 σc,0(top-left) Ee,k 1 yc,(top-left) −xc,(top-left) εk − εsh,k + ⎧ ⎫ ⎡ ⎤ −6 ⎨ ⎬ −592.0 × 10−6 ⎦ − −400 × 10−6 = 13,910 × 1 −200 −(−150) ⎣ 1.058 × 10 ⎩ ⎭ 1.903 × 10−6 + (−0.304) (−2.79) = −0.79 MPa σc,k(top-right) = −6.49 MPa σc,k(btm-right) = −2.28 MPa σc,k(btm-left) = 3.42 MPa σs(1),k = Es 1 ys(1) −xs(1) εk

⎤ −592.0 × 10−6 = 200 × 103 × 1 −150 −(−90) × ⎣ 1.058 × 10−6 ⎦ 1.903 × 10−6 = −115.9 MPa; σs(2),k = −184.4 MPa σs(3),k = −84.1 MPa σs(4),k = −152.7 MPa σs(5),k = −52.4 MPa σs(6),k = −120.8 MPa

⎡

Stresses and strains calculated at time τk are shown in Fig. 6.9. Signiﬁcant transfer of axial compressive load took place from the concrete to the steel with time, with the maximum compressive stress in the concrete reducing from −10.18 MPa at τ0 to −6.49 MPa at τk and the compressive stress in the most heavily stressed reinforcing bar increasing from −50.1 MPa to −184.4 MPa. It is also noted that the tensile stress in the concrete in the bottom left corner of the cross-section has increased from 2.73 MPa to 3.42 MPa, indicating that cracking may well occur during a period of sustained loading (primarily due to shrinkage). The slopes of the applied moment Me,k and the neutral axis are (Eqs 6.4 and 6.45a): tan θM,k = tan θM,0 = 1.0 and therefore θM,k = 45◦ and tan θNA,k =

κy,k κx,k

=

1.903 × 10−6 = 1.80 and therefore θNA,k = 60.91◦ . 1.058 × 10−6

The neutral axis passes through the y-axis at (Eq. 6.45b): y=−

εr,k −592.0 × 10−6 =− = 559.2 mm κx,k 1.058 × 10−6

This indicates a translation of the neutral axis with a slight rotation from the results previously obtained at time τ0 . In fact, the slope of the neutral axis varies

Uncracked sections 251

60.91°

x 45° −1089.3 × 10−6

Me,k

y Neutral axis −184.4 −6

−94.7 × 10

−152.7 −120.9 −115.9

e

−6.49

−84.1 −52.4

σ

3.42

Figure 6.9 Final strain and stress diagrams at time τk (Example 6.4) (all units in mm, MPa).

from θNA,0 = 60.76◦ to θNA,k = 60.91◦ while the intersection with the y-axis moves from y = 270.2 mm at τ0 to y = 559.2 mm at τk . The translation of the neutral axis is mostly due to the effects of shrinkage. If the example was repeated with shrinkage set to zero, the intersection with the y-axis would change only slightly from y = 270.2 mm at τ0 to y = 275.3 mm at τk .

Example 6.5 The long-term strains and stresses on the cross-section of Fig. 6.7 are to be determined using the AEMM assuming that the external loads applied in Example 6.3 (i.e. Ne = −800 kN, Mxe = 50 kNm, Mye = 25 kNm) are to be

252 Uncracked sections sustained between times τ0 and τk . The instantaneous material properties are the same as in Example 6.3: Ec,0 = 32 GPa, Es = 200 GPa, and ns,0 = Es /Ec,0 = 6.25. The creep coefﬁcient, ageing coefﬁcient and shrinkage strain associated with the time period τ0 to τk are: ϕ(τk , τ0 ) = 2.0; χ (τk , τ0 ) = 0.65 and εsh (τk ) = − 400 × 10−6 . From Example 6.3 at τ0 : εr,0 = −115.3 × 10−6 ; κx0 = 0.378 × 10−6 mm−1 ; κy0 = 0.111 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 32,000 = = 13,910 MPa 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.0 and therefore n¯ s,k = 14.38

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.0 × (0.65 − 1.0) Fe,0 = = −0.304 = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.0 and for this reinforced concrete section, the vectors re,k , fp,init and fp.rel,k in Eq. 6.41 are: ⎡ ⎤ −800 × 103 N re,k = ⎣ 50 × 106 Nmm ⎦ 25 × 106 Nmm ⎡ ⎤ 0N fp,init = ⎣ 0 Nmm ⎦ 0 Nmm ⎡ ⎤ 0N fp.rel,k = ⎣ 0 Nmm ⎦ 0 Nmm The properties of the age-adjusted transformed cross-section based on Ee,k are: ¯ k = bD − b2 D2 + (n¯ s,k − 1) A

8 0

As(i) = 246.2 × 103 mm2

i=1

D1 D2 B¯ x,k = bD1 − dy.ref + b1 D2 D1 + − dy.ref 2 2 8 0 As(i) ys(i) = 62.69 × 103 mm3 + (n¯ s,k − 1)

i=1

8 0 b b1 B¯ y,k = bD1 As(i) xs(i) − dx.ref + b1 D2 − dx.ref + (n¯ s,k − 1) 2 2 i=1 = 62.69 × 103 mm3

2

2 bD31 b1 D32 D1 D2 ¯Ix,k = − dy.ref + − dy.ref + bD1 + b1 D2 D1 + 2 2 12 12 8 0 2 = 4439 × 106 mm4 + (n¯ s,k − 1) As(i) ys(i) i=1

2

D2 b31 D1 b3 b I¯y,k = + bD1 − dx.ref + + b1 D2 12 2 12 8 0 + (n¯ s,k − 1) As(i) x2s(i) = 4439 × 106 mm4

Uncracked sections 253

2 b1 − dx.ref 2

i=1

b D2 ¯Ixy,k = bD1 D1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref + (n¯ s,k − 1) As(i) xs(i) ys(i) = −1067 × 106 mm4 × 2 i=1 The geometric properties of the concrete are required to evaluate f cr,k and f sh,k : Ac = bD − b2 D2 − Bxc = bD1

8 0

As(i) = 194.4 × 103 mm2

i=1

D1 − dy.ref 2

8 0 D2 + b1 D2 D1 + As(i) ys(i) − dy.ref − 2 i=1

= −35.64 × 103 mm3

8 0 b b1 Byc = bD1 − dx.ref + b1 D2 − dx.ref − As(i) xs(i) 2 2 i=1 = −35.64 × 103 mm3

2

2 bD31 b1 D32 D1 D2 Ixc = + bD1 − dy.ref + + b1 D2 D1 + − dy.ref 12 2 12 2 −

8 0 i=1

Iyc =

2 = 3417 × 106 mm4 As(i) ys(i)

2

2 D2 b31 b b1 D1 b3 + bD1 − dx.ref + + b1 D2 − dx.ref 12 2 12 2 −

8 0 i=1

As(i) x2s(i) = 3417 × 106 mm4

D1 b D2 Ixyc = bD1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref − As(i) xs(i) ys(i) = −831.9 × 106 mm4 × 2 i=1 From Eqs 6.39c and d: ⎡

⎤

⎡

⎤ 218.3 × 103 N ⎢ ⎥ ⎢ ⎥ fcr,k = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ = ⎣ −13.52 × 106 Nmm ⎦ −6.705 × 106 Nmm −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 Ac εr,0 + Bxc κx,0 − Byc κy,0

254 Uncracked sections ⎡

⎤ ⎡ ⎤ 194.4 × 103 Ac fsh,k = ⎣ Bxc ⎦ Ee,k εsh,k = ⎣ −35.64 × 103 ⎦ × 13,910 × −400 × 10−6 −Byc 35.64 × 103 ⎡ ⎤ −1082 × 103 N = ⎣ 0.198 × 106 Nmm ⎦ −0.198 × 106 Nmm Based on properties of the age-adjusted transformed cross-section, Fk is calculated using Eq. 6.42a, except that the age-adjusted modulus Ee,k is used instead of Ec,0 : ⎡

2.920×10−10

⎢ Fk = ⎣ −5.429×10−15 5.429×10−15

−5.429×10−15 1.719×10−14 −4.133×10−15

5.429×10−15

⎤

⎥ −4.133×10−15 ⎦ 1.719×10−14

The strain εk at time τk is obtained using Eq. 6.41: ⎡

⎤ −613.4 × 10−6 εk = Fk (re,k − fcr,k + fsh,k ) = ⎣ 0.976 × 10−6 mm−1 ⎦ 0.267 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,k = −613.4 × 10−6 κx,k = 0.976 × 10−6 mm−1 κy,k = 0.267 × 10−6 mm−1 The strains at the corners of the cross-section are obtained from Eq. 6.1: εk(corner 1) = −766.4 × 10−6 εk(corner 2) = −894.4 × 10−6 εk(corner 3) = −601.6 × 10−6 εk(corner 4) = −553.5 × 10−6 εk(corner 5) = −377.8 × 10−6 εk(corner 6) = −297.8 × 10−6 and the corresponding concrete stresses are obtained using Eq. 6.43a: ' 1 ycorner 1 −xcorner 1 εk − εsh,k + Fe,0 σc,0(corner 1) = −3.41 MPa σc,k(corner 2) = −4.68 MPa σc,k(corner 3) = −1.71 MPa

σc,k(corner 1) = Ee,k

&

Uncracked sections 255 σc,k(corner 4) = −1.23 MPa σc,k(corner 5) = 0.55 MPa σc,k(corner 6) = 1.34 MPa The strains in the steel reinforcing bars are: εs(1),k = −723.8 × 10−6 εs(2),k = −771.9 × 10−6 εs(3),k = −819.9 × 10−6 εs(4),k = −548.1 × 10−6 εs(5),k = −596.1 × 10−6 εs(6),k = −644.1 × 10−6 εs(7),k = −372.4 × 10−6 εs(8),k = −420.4 × 10−6 and from Eq. 6.43b, the steel stresses are: σs(1),k = −144.8 MPa σs(2),k = −154.4 MPa σs(3),k = −164.0 MPa σs(4),k = −109.6 MPa σs(5),k = −119.2 MPa σs(6),k = −128.8 MPa σs(7),k = −74.5 MPa σs(8),k = −84.1 MPa The slope of the applied moment Me,k is calculated based on Eq. 6.4 at time τk : tan θM,k =

Mye,k Mxe,k

=

25 × 106 = 0.5 and therefore θM,k = 26.56◦ 50 × 106

The equation of the line of the neutral axis at time τk (in the x-y plane) is from Eq. 6.44: y=

κy,k κx,k

x−

εr,k 0.267 × 10−6 −613.4 × 10−6 = x − = 0.273x + 628.3 κx,k 0.976 × 10−6 0.976 × 10−6

and with tan θNA,k = 0.273, the inclination of the neutral axis is θNA,k = 15.28◦ and it passes through the y-axis at y = 628.3 mm. Without shrinkage, the intersection with the y-axis occurs at y(x = 0) = 307.9 mm (close to the value of 304.8 mm calculated at time τ0 ).

256 Uncracked sections The ﬁnal stresses and strains on the cross-section are shown in Fig. 6.10. 15.28° −894.4 × 10−6 −4.68

−164.0 −154.4

x

−144.8 Me,k

26.56°

−128.8 −119.2 −109.6

−84.1

y −297.8 × 10−6

−74.5 e

1.34

s

Figure 6.10 Final strain and stress diagrams at time τk for Example 6.5 (all units in mm, MPa).

6.4 Long-term analysis using the step-by-step method The use of the SSM is particularly useful for the long-term analysis of reinforced concrete columns as it enables complex loading histories to be considered, such as those that occur during different construction stages. It also permits improved accuracy with ﬁner time discretisation. In the following, only the steps peculiar to combined axial force and biaxial moments are presented as the use of the SSM has been extensively discussed in Chapters 4 and 5. When using the SSM the time domain is discretised into a number of instants τj , with j = 1, . . ., k and with τk being the instant at which the long-term response is sought. The constitutive relationships for the concrete and the steel reinforcement and tendons are deﬁned in Eqs 4.25 and 5.44. The solution process is similar to that already outlined for both the instantaneous analysis and time analysis using the AEMM. At any time instant τj , the problem is expressed in terms of the three variables that deﬁne the strain diagram (εr,j , κx,j and κy,j ) and these are determined based on equilibrium considerations written as: re,j = ri,j

(6.47)

Uncracked sections 257 where re,j and ri,j represent the external and internal actions, and similarly to Eq. 5.46, may be expressed by: T re,j = Ne,j Mxe,j Mye,j

(6.48a)

T ri,j = Ni,j Mxi,j Myi,j

(6.48b)

and

The internal actions ri,j are expressed in terms of the strain measured at the origin of the reference system (εr,j ), and the curvatures calculated with respect to the x- and y-axes (κx,j and κy,j ). Using the constitutive relationships speciﬁed in Eqs 4.25 and 5.44, the contribution to the internal axial force carried by the concrete, the steel reinforcement and the tendons at time τj may be written as:

Nc,j =

σc,j dA = Ac

⎡

⎤ j−1 ⎣Ec,j εr,j + yκx,j − xκy,j − εsh,j + Fe,j,i σc,i ⎦ dA i=0

Ac

= Ac Ec,j εr,j + Bxc Ec,j κx,j − Byc Ec,j κy,j − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

(6.49a)

i=0

Ns,j = RA,s εr,j + RBx,s κx,j − RBy,s κy,j Np,j = RA,p εr,j + RBx,p κx,j − RBy,p κy,j +

(6.49b) mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.49c)

i=1

where the cross-sectional rigidities have been introduced previously in Eqs 6.7, 6.10 and 6.13. The expression for Ni,j (included in ri,j ) can be obtained by summing Eqs 6.49: Ni,j = RA,j εr,j + RBx,j κx,j − RBy,j κy,j − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

i=0

+

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50a)

i=1

Similarly, the expressions for the internal moments are given by: Mxi,j = RBx,j εr,j + RIx,j κx,j − RIxy,j κy,j − Bxc Ec,j εsh,j +

j−1

Fe,j,i Mxc,i

i=0

+

mp i=1

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50b)

258 Uncracked sections Myi,j = −RBy,j εr,j − RIxy,j κx,j + RIy,j κy,j + Byc Ec,j εsh,j +

j−1

Fe,j,i Myc,i

i=0 mp

−

xp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50c)

i=1

where the cross-sectional rigidities are determined using Eqs 6.15 (proposed for the instantaneous analysis) except that the concrete elastic modulus at time τj , Ec,j , is used instead of the instantaneous value at time τ0 , Ec,0 . The equilibrium equations of Eqs 6.47 can be expressed in compact form at time τj as: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j

(6.51)

where: ⎡

⎤ εr,j εj = ⎣ κx,j ⎦ κy,j ⎡ ⎤ RBx,j −RBy,j RA,j RIx,j −RIxy,j ⎦ Dj = ⎣ RBx,j −RBy,j −RIxy,j RIy,j fcr,j =

j−1

Fe,j,i rc,i

(6.52a)

(6.52b)

(6.52c)

i=0

⎡

⎤ Ac fsh,j = ⎣ Bxc ⎦ Ec,j εsh,j −Byc ⎡ ⎤ mp Ap(i) Ep(i) εp(i),init ⎢ ⎥ fp,init = ⎣ yp(i) Ap(i) Ep(i) εp(i),init ⎦ i=1 −xp(i) Ap(i) Ep(i) εp(i),init ⎡ ⎤ mp Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) ⎢ ⎥ fp.rel,j = ⎣ yp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) ⎦ i=1 −xp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init )

(6.52d)

(6.52e)

(6.52f)

where rc,i included in the calculation of f cr,j depicts the internal actions resisted by the concrete part of the cross-section at time τi (for which i < j) and is calculated based on: ⎡

⎤ ⎡ ⎤ i−1 Nc,i Ac rc,i = ⎣ Mxc,i ⎦ = Dc,i εi + Fe,i,n rc,n − ⎣ Bxc ⎦ Ec,i εsh,i = Dc,i εi + fcr,i − fsh,i Myc,i −Byc n=0 (6.53)

Uncracked sections 259 in which ⎤ Ac Bxc −Byc ⎥ ⎢ Dc,i = ⎣ Bxc Ixc −Ixyc ⎦ Ec,i −Byc −Ixyc Iyc ⎡

(6.54)

The strain diagram at time τj can then be determined based on: εj = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j

(6.55)

in which Fj is identical to F0 (deﬁned in Eqs 6.19), except that concrete elastic modulus Ec,j replaces Ec,0 . The stress distribution at time τk can then be calculated substituting the expression for the strain εk = εr,k + yκx,k − xκy,k = 1 y −x εk into Eqs 5.60. The simpliﬁcations proposed for doubly-symmetric columns previously introduced for the instantaneous analysis and for the time analysis using the AEMM, can also be applied at time τj when using the SSM. As in the previous analyses, the cross-sectional rigidities included in Fj could be calculated based on the transformed concrete cross-section obtained using the appropriate modular ratios ns(i),j = Es(i) /Ec,j and np(i),j = Ep(i) /Ec,j for the i-th steel bar and the i-th tendon, respectively.

7

Cracked sections

7.1 Introductory remarks In the cross-sectional analyses of Chapters 4, 5 and 6, it was assumed that concrete can carry imposed stresses, both compressive and tensile. However, in reality concrete is not able to carry large tensile stress. If the tensile stress at a point reaches the tensile strength of concrete (Eq. 2.1), cracking occurs. Cracking is irreversible. On a cracked cross-section, tensile stress of any magnitude cannot be carried normal to the crack surface at any time after cracking and tensile forces can only be carried across a crack by steel reinforcement. Therefore, on a cracked cross-section, internal actions can be carried only by the steel reinforcement (and tendons) and the uncracked parts of the concrete section. In members subjected only to axial tension, caused either by external loads or by restraint to shrinkage or temperature change, full-depth cracks occur when the tensile stress is exceeded (i.e. at each crack location, the entire cross-section is cracked). When the axial tension is caused by restraint to shrinkage, cracking causes a loss of stiffness and a consequent decrease in the internal tension. The crack width and the magnitude of the restraining force, as well as the spacing between the cracks, depend on the amount of bonded reinforcement. Between the cracks in a member subjected to axial tension, the concrete continues to carry tensile stress and hence continues to contribute to the member stiffness. This is the tension stiffening effect and was discussed in Section 3.6.2. When cracking occurs in ﬂexural members and the tensile strength of the concrete on the tensile surface of the member is reached, primary cracks develop at regular spacing on the tensile side of the member, as shown in Fig. 3.4a. A sudden loss of stiffness occurs at ﬁrst cracking and the short-term moment–curvature relationship becomes nonlinear. The primary cracks penetrate spontaneously to a height ho (see Fig. 3.4a) which depends on the quantity of steel and the magnitude of any axial force or prestress. For reinforced concrete members in pure bending with no axial force, the height of the primary cracks ho immediately after cracking is usually relatively high (0.6 to 0.9 times the depth of the member) and remains approximately constant under increasing bending moments until either the steel reinforcement yields or the concrete stress–strain relationship in the compressive region becomes non-linear. For prestressed members and members subjected to bending plus axial compression, ho may be relatively small initially and gradually increases as the applied moment increases, even when material behaviour is linear-elastic.

Cracked sections 261 The stress in the tensile reinforcement and the stress in the concrete at the steel level for the cracked member of Fig. 3.4a are illustrated in Figs 3.4b and c, respectively. Immediately after ﬁrst cracking, the intact concrete between adjacent primary cracks carries considerable tensile force, mainly in the direction of the reinforcement, due to the bond between the steel and the concrete. The average tensile stress in the concrete is a signiﬁcant percentage of the tensile strength of concrete. The steel stress is a maximum at a crack, where the steel carries the entire tensile force, and drops to a minimum between the cracks, as shown (Fig. 3.4b). The bending stiffness of the member is considerably greater than that based on a fully-cracked section, where concrete in tension is assumed to carry zero stress. This tension stiffening effect may be signiﬁcant in the service-load performance of beams and even more so for lightly reinforced slabs. The Euler–Bernoulli assumption that plane sections remain plane is not strictly true for a cross-section in the cracked region of a beam. However, if strains are measured over a gauge length containing several primary cracks, the average strain diagram is linear over the depth of the member. As the load increases above the cracking moment Mcr , and after the primary cracks have developed, secondary cracks (or cover-controlled cracks) form around the reinforcement between the primary cracks, the average concrete tensile stress drops and the tension stiffening effect gradually reduces. A typical moment versus average curvature relationship for a reinforced concrete cross-section in pure bending is shown in Fig. 7.1a as the solid line OAB in which Ms represents the applied service moment. Also shown as the dashed line OC of slope (EI)cr is the moment–curvature relationship for a fully-cracked cross-section. As moment increases after ﬁrst cracking, the ﬂexural rigidity gradually reduces from that of the uncracked section (EI)uncr at ﬁrst cracking and approaches that of the fully-cracked section, (EI)cr , as the moment becomes large, as shown. If an uncracked singly reinforced member such as that shown in Fig. 1.14a begins to shrink prior to loading, as is commonly the case, shrinkage warping occurs and a shrinkage-induced curvature κsh.uncr develops on the uncracked cross-section when the applied moment is still zero (i.e. Ms = 0) as shown in Fig. 7.1b as point O . The curvature κsh.uncr and the tensile stress caused by shrinkage in the extreme ﬁbre of the uncracked cross-section σcs were illustrated in Fig. 1.14b. Because of the initial tensile stress σcs in the concrete, the moment required to cause ﬁrst cracking Mcr.sh0 will be less than Mcr (as indicated in Fig. 7.1) and the moment-curvature relationship is now represented by curve O A B in Fig. 7.1b. The initial curvature due to early shrinkage on a fully-cracked cross-section (κsh.cr ) where the concrete is assumed to carry no tension is signiﬁcantly larger that that of the uncracked member (κsh.uncr ), as illustrated in Fig. 1.14. Therefore, early shrinkage before loading causes the dashed line representing the fully-cracked response to move further to the right, shown as line O C in Fig. 7.1b. For a prestressed concrete member, or a reinforced concrete member in combined bending and compression, the effect of tension stiffening is less pronounced because the loss of stiffness of the cracked section is less dramatic. As the applied moment increases, the depth of the primary cracks increases gradually (in contrast to the sudden crack propagation in a reinforced member in pure bending) and the depth of the concrete compressive zone is signiﬁcantly greater than would be the case if no axial force was present. A typical short-term moment-average curvature relationship for a

262 Cracked sections Tension stiffening, dk Moment

B Average M vs k

C

(EI )cr

(EI)uncr

Concrete carries no tension anywhere

Ms A

Mcr

Uncracked cross-section Curvature, k

O

(a) No shrinkage prior to loading B′ C′

Tension stiffening, dk

Moment

Average M vs k (EI )cr

(EI )uncr Ms

Concrete carries no tension anywhere

A′

Mcr.sh0

Uncracked cross-section O′ O ksh.uncr

O″ Curvature, k ksh.cr (b) Shrinkage strain esh,0 prior to loading

Figure 7.1 Moment-average curvature relationship for a reinforced concrete cross-section at ﬁrst loading, τ0 .

prestressed concrete cross-section containing bonded tensile reinforcement is shown in Fig. 7.2, together with the moment–curvature relationship for the cross-section containing a crack. The internal moment caused by the resultant prestressing force about the centroidal axis of the uncracked section is designated Pe. As can be seen by comparing the curves in Figs 7.1a and 7.2, the presence of the axial prestress signiﬁcantly changes the shape of curve after cracking. The prestressing force (or axial compression) increases the post-cracking stiffness and greatly improves the in-service behaviour of a concrete member after the onset of ﬂexural cracking. In Section 3.6.3, modular ratio theory was presented for the determination of the stresses and deformations of a singly-reinforced rectangular cross-section in pure

Cracked sections 263 M − Pe

Average M vs k

Concrete carries no tension anywhere

Slope of tangent = (EI)cr

M

Mcr

(EI)uncr Curvature, k

−Pe

Figure 7.2 Short-term moment-average curvature relationship for a prestressed concrete cross-section.

bending at a primary crack location. The properties of the fully-cracked cross-section, including the depth to the neutral axis kd (Eq. 3.14) and the second moment of area of the cracked section about its centroidal axis Icr (Eq. 3.17) were also derived. For a more general cross-section, the properties of the cracked section may be determined from a transformed section analysis in which the tensile concrete is ignored. Such an analysis is presented in Section 7.2. Cracking also inﬂuences the time-dependent behaviour of reinforced and prestressed concrete members. In Section 1.2.7, the effects of creep on a fully-cracked cross-section were compared with the corresponding effects on an uncracked cross-section (see Fig. 1.12), while the stresses and deformations caused by shrinkage on a cracked section were discussed in Section 1.3.3 and illustrated in Fig. 1.14b. For a cross-section subjected to constant sustained moment over the time period τ0 to t, if no shrinkage has occurred prior to loading, the instantaneous moment versus curvature response of the cross-section is shown as curve OAB in Fig. 7.3a (identical to curve OAB in Fig. 7.1a). The instantaneous fully-cracked section response (calculated ignoring the tensile concrete) is shown as dashed line OC in Fig. 7.3a. If the crosssection does not shrink with time (i.e. εsh remains at zero), creep causes an increase in curvature with time at all moment levels and the time-dependent M − κ response shifts to curve OA B in Fig. 7.3a. The creep-induced increase in curvature with time may be expressed as κcr (t) = κi ϕ(t, τ0 )/α, where κi is the instantaneous curvature, ϕ(t, τ0 ) is the creep coefﬁcient and α is a factor that depends on the amount of cracking and the reinforcement quantity and location. Approximate expressions for α were given in Eqs 3.32 and, for typical reinforcement ratios for beams and slabs, α is in the range 1.0– 1.3 prior to cracking and in the range 4–6 when cracking is extensive. With regard to the response of a fully-cracked cross-section (calculated ignoring the tensile concrete), creep causes a softening of the response shown as dashed line OC in Fig. 7.3a, with the slope of the line decreasing by the factor 1/(1 + ϕ(t, τ0 )/α), where α is in the range 4–6 depending on the reinforcement ratio.

264 Cracked sections Moment

B

B′

C

C′

Instantaneous member response D

M1

D′

E

A

Mcr

E′

Member response after creep at time t

A′

Fully-cracked response after creep at time t Instantaneous response of fullycracked section Curvature, k O

ki + Δk cr(t)

ki

(a) Effects of creep (zero shrinkage)

B

Moment

B′ C′

C

Instantaneous member response D

M1

D′

E

E′

A

Mcr

Member response after creep and shrinkage at time t

A′

Mcr.sh

Fully-cracked response after creep and shrinkage at time t Curvature, k O

O′

O″

ki

ki + Δkcr(t) + Δksh(t)

(b) Effects of creep and shrinkage

Figure 7.3 Moment-average curvature relationship for a reinforced concrete cross-section under sustained loads at time t.

When shrinkage before and after ﬁrst loading is included, the curvature increases even further with time and the time-dependent response of the cross-section is shown as curve O A B in Fig. 7.3b. At M = 0, the curvature increases due to shrinkage of the uncracked cross-section and the point O moves horizontally to O . Due to the restraint to shrinkage provided by the bonded reinforcement, tensile stress is induced with time and this has the effect of lowering the cracking moment from Mcr to Mcr.sh , as shown in Fig. 7.3b. For any cross-section subjected to a sustained moment in the range Mcr.sh < M ≤ Mcr , cracking will occur with time and the increase in curvature will be exacerbated by the loss of stiffness caused by time-dependent cracking. In practice, critical sections of many lightly reinforced slabs are loaded in this range.

Cracked sections 265 The response of the cracked section (ignoring the tensile concrete) after creep and shrinkage is shown as line O C in Fig. 7.3b. The shrinkage-induced curvature of the fully-cracked cross-section when M = 0 is greater than that of the uncracked crosssection and the cracked section response is shifted horizontally from point O to point O , as shown. The slope of the cracked section response in Fig. 7.3b is softened by creep and the slope of the line O C in Fig. 7.3b is the same as the slope of line OC in Fig. 7.3a. At a typical in-service moment M1 , the instantaneous curvature due to tension stiffening κ ts.0 is DE in Fig. 7.3b and the time-dependent tension stiffening curvature after the period of sustained loadings κ ts (t) is D E in Fig. 7.3b. Tension stiffening reduces under sustained loading, primarily due to time-dependent cracking, shrinkageinduced degradation of bond at the concrete-reinforcement interface and tensile creep between the cracks in the tensile concrete. It is generally believed that tension stiffening reduces rapidly after ﬁrst loading and reduces to about half its instantaneous value with time (Refs 1–4). When a fully-cracked cross-section is subjected to a period of sustained loading, creep causes a change in position of the neutral axis. In general, the depth to the neutral axis increases with time and, hence, so too does the area of concrete in compression. To account accurately for this gradual change of the properties of the cross-section, an iterative numerical solution procedure is required, in which the time period is divided into small increments and the cross-sectional properties at the end of each time increment are modiﬁed. While such a procedure is routinely implemented in ﬁniteelement models of cracked reinforced concrete, often using a layered cross-section, it is not suitable for manual solution. The time analysis of a cracked cross-section using the age-adjusted effective modulus method is presented in Section 7.3. In this analysis, the dimensions of the fully-cracked cross-section are assumed to remain constant throughout the time analysis, i.e. the depth of the concrete in compression and the extent of cracking are assumed to remain constant with time. This assumption is in fact necessary, if the short-term and time-dependent stress and strain increments are to be calculated separately and added together to obtain ﬁnal stresses and deformations, i.e. if the principle of superposition is to be applied to fully-cracked sections in the same way as it has been applied to uncracked cross-sections. The assumption also greatly simpliﬁes the analysis and usually results in relatively little error in the estimation of time-dependent deformations.

7.2 Short-term analysis In this section, the short-term responses of fully-cracked reinforced and partiallyprestressed concrete cross-sections subjected to combined bending and axial force are considered. The time-dependent effects of creep and shrinkage are considered in Section 7.3. As for the analyses of uncracked cross-sections in Chapters 4, 5 and 6, the analysis presented here is based on the following assumptions: • •

Plane sections remain plane and, as a consequence, the strain distribution is linear over the depth of the section. Perfect bond exists between the steel and the concrete, i.e. steel and concrete strains are assumed to be compatible. This is usually a reasonable assumption at service loads in members containing deformed steel reinforcing bars and strands.

266 Cracked sections • •

Tensile stress in the concrete is ignored, and therefore the tensile concrete does not contribute to the cross-sectional properties. Material behaviour is linear-elastic. This includes concrete in compression, and both the non-prestressed and prestressed reinforcement.

The two cases of axial force with uniaxial bending and axial force with biaxial bending are dealt with separately in the following sections. 7.2.1 Axial force and uniaxial bending In the short-term analysis of the section at ﬁrst loading (at time τ 0 ), it is assumed that the axial force and bending moment about the x-axis, Ne,0 and Me,0 , respectively, produce tension of sufﬁcient magnitude to cause cracking in the bottom ﬁbres of the cross-section and compression at the top of the section. Consider the cracked partially-prestressed concrete cross-section shown in Fig. 7.4. The section is symmetric about the y-axis and, for convenience, the orthogonal x-axis is selected as the reference axis. Also shown in Fig. 7.4 are the initial stress and strain distributions when the section is subjected to combined bending and axial force (Me.0 and Ne.0 ) sufﬁcient to cause cracking in the bottom ﬁbres. The numbers of layers of non-prestressed and prestressed reinforcement for the cross-section in Fig. 7.4 are ms = 3 and mp = 2, respectively. As for the analysis of uncracked cross-sections in Section 5.3, the properties of each layer of non-prestressed reinforcement are deﬁned by its area, elastic modulus and location with respect to the arbitrarily chosen x-axis, i.e. As(i) , Es(i) and ys(i) (= ds(i) − dref ), respectively. Similarly, Ap(i) , Ep(i) and yp(i) (= dp(i) − dref ) represent the area, elastic modulus and location of the prestressing steel with respect to the x-axis, respectively. The strain at any depth y below the reference x-axis at time τ 0 is given by: ε0 = εr,0 + yκ0

(7.1)

The stresses in the concrete and in the bonded reinforcement are: σc,0 = Ec,0 ε0 = Ec,0 (εr,0 + yκ0 ) for y ≤ yn,0

(7.2a)

σc,0 = 0 for y > yn,0

(7.2b)

ds(1) ds(2)

dref ys(1) ys(2)

As(1) As(2) x

yn,0 dp(1) dp(2)

ds(3)

yp(1) yp(2) ys(3)

Ap(1) Ap(2) As(3)

etop es(1) es(2)

Me,0 Ne,0

eref

stop = Ec,0etop

e

ss(1) ss(2)

s

sp(1) sp(2) ss(3)

es(3)

y (a) Cross-section

(b) Strain diagram

(c) Stress

Figure 7.4 Fully-cracked reinforced concrete cross-section.

Cracked sections 267 σs(i),0 = Es(i) ε0 = Es(i) (εr,0 + ys(i) κ0 ) σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) εr,0 + yp(i) κ0 + εp(i),init

(7.3) (7.4)

where yn,0 is the distance from the reference axis to neutral axis, as shown in Fig. 7.4a, and εp(i),init is the strain in the i-th layer of prestressing steel immediately before the transfer of prestress to the concrete as expressed in Eq. 5.5 (reproduced and renumbered here for convenience): Pp(i),init Ap(i) Ep(i)

εp(i),init =

(7.5)

The internal axial force Ni,0 on the cracked cross-section is the sum of the axial forces resisted by the various materials forming the cross-section and is given by: Ni,0 = Nc,0 + Ns,0 + Np,0

(7.6)

where Nc,0 , Ns,0 and Np,0 represent the axial forces resisted by the concrete, the nonprestressed reinforcement and the prestressing steel, respectively, and are calculated using: Nc,0 =

σc,0 dA =

Ac

Ns,0 =

Ec,0 (εr,0 +yκ0 ) dA = Ac Ec,0 εr,0 +Bc Ec,0 κ0

(7.7a)

Ac

ms

ms ms As(i) Es(i) εr,0 +ys(i) κ0 = As(i) Es(i) εr,0 + ys(i) As(i) Es(i) κ0

i=1

i=1

i=1

(7.7b) mp mp mp Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(i) Ep(i) εp(i),init Np,0 = i=1

i=1

(7.7c)

i=1

where Ac and Bc are the area and the ﬁrst moment of area about the x-axis of the compressive concrete above the neutral axis (i.e. the properties of the intact compressive concrete). Adopting the following notation: RA,s =

ms ms ms 2 As(i) Es(i) ;RB,s = ys(i) As(i) Es(i) ;RI,s = ys(i) As(i) Es(i) i=1

RA,p =

i=1

i=1

mp mp mp 2 Ap(i) Ep(i) ;RB,p = yp(i) Ap(i) Ep(i) ;RI,p = yp(i) Ap(i) Ep(i) i=1

i=1

(7.8)

i=1

Eqs 7.7 become Nc,0 =

σc,0 dA =

Ac

Ec,0 (εr,0 + yκ0 )dA

(7.9a)

Ac

Ns,0 = RA.s εr,0 + RB.s κ0

(7.9b)

268 Cracked sections Np,0 = RA,p εr,0 + RB,p κ0 +

mp Ap(i) Ep(i) εp(i),init

(7.9c)

i=1

Remembering that for equilibrium Ne,0 = Ni,0 and that substituting Eqs 7.9 into Eq. 7.6 the expression for Ni,0 can be re-written in terms of the actual geometry and the elastic moduli of the materials forming the cross-section: Ni,0 =

Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 + (RB,s + RB,p )κ0 Ac

+

mp Ap(i) Ep(i) εp(i),init = Ne,0

(7.10)

i=1

Eq. 7.10 can be re-expressed as: mp Ne,0 − Ap(i) Ep(i) εp(i),init = Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 i=1

Ac

+ (RB,s + RB,p )κ0

(7.11)

Similarly, the following expression based on moment equilibrium can be derived as: mp Me,0 − yp(i) Ap(i) Ep(i) εp(i),init = Ec,0 (εr,0 + yκ0 )ydA + (RB,s + RB,p )εr,0 i=1

Ac

+ (RI,s + RI,p )κ0

(7.12)

For a reinforced concrete section comprising rectangular components (e.g. rectangular ﬂanges and webs) loaded in pure bending (i.e. Ne,0 = Ni,0 = 0) and with no prestress, Eq. 7.10 becomes a quadratic equation that can be solved to obtain the location of the neutral axis yn,0 . If the cross-section is prestressed or the axial load Ne,0 is not equal to zero, dividing Eq. 7.12 by Eq. 7.11 gives: Me,0 −

mp 0

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

(Ap(i) Ep(i) εp(i),inst )

i=1 y=y 1 n,0

=

Ec,0 (εr,0 + yκ0 )ydA + (RB,s + RB,p )εr,0 + (RI,s + RI,p )κ0

y=−dref y=y 1 n,0 y=−dref

Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 + (RB,s + RB,p )κ0

Cracked sections 269 Dividing top and bottom of the right hand side by κ 0 and recognising that at the axis of zero strain y = yn,0 = −εr,0 /κ0 , the above expression becomes: Me,0 −

mp 0

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

(Ap(i) Ep(i) εp(i),inst )

i=1 y=y 1 n,0

=

Ec,0 (−yn,0 + y)ydA − (RB,s + RB,p )yn,0 + (RI,s + RI,p )

y=−dref y=y 1 n,0

(7.13) Ec,0 (−yn,0 + y)dA − (RA,s + RA,p )yn,0 + (RB,s + RB,p )

y=−dref

and Eq. 7.13 may be solved for yn,0 relatively quickly using a simple trial and error search. When yn,0 is determined, and the depth of the intact compressive concrete above the cracked tensile zone is known, the properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis may be readily calculated. Using the same notation as in the short-term analysis of the uncracked section of Section 5.3 (Eqs 5.8–5.11), the expressions for Ni,0 and Mi,0 (Eqs 7.10 and 7.12) can be rewritten as: Ni,0 = RA,0 εr,0 + RB,0 κ0 +

mp Ap(i) Ep(i) εp(i),init

(7.14a)

i=1 mp

Mi,0 = RB,0 εr,0 + RI,0 κ0 +

yp(i) Ap(i) Ep(i) εp(i),init

(7.14b)

i=1

and RA,0 , RB,0 and RI,0 are the axial rigidity and the stiffness related to the ﬁrst and second moments of area of the cracked section about the reference axis, respectively, calculated at time τ 0 and are given by: RA,0 = Ac Ec,0 +

ms i=1

RB,0 = Bc Ec,0 +

ms

As(i) Es(i) +

mp

Ap(i) Ep(i) = Ac Ec,0 + RA,s + RA,p

(7.15a)

i=1

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i) = Bc Ec,0 + RB,s + RB,p

i=1

(7.15b) RI,0 = Ic Ec,0 +

ms i=1

mp

2 ys(i) As(i) Es(i) +

2 yp(i) Ap(i) Ep(i) = Ic Ec,0 + RI,s + RI,p (7.15c)

i=1

The system of equilibrium equations governing the problem (Eq. 5.12) is rewritten here as: re,0 = D0 ε0 + fp,init

(7.16)

270 Cracked sections and solving gives the vector of unknown strains: re,0 − fp,init = F0 re,0 − fp,init ε0 = D−1 0

(7.17)

As deﬁned previously:

Ne,0 re,0 = Me,0

RB,0 RI,0

RA,0 D0 = RB,0

εr,0 ε0 = κ0 fp,init =

mp i=1

F0 =

(7.18a) (7.18b)

(7.18c) Ap(i) Ep(i) εp(i),init yp(i) Ap(i) Ep(i) εp(i),init

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

(7.18d) −RB,0 RA,0

(7.18e)

The stress distribution in the concrete and reinforcement can then be calculated from Eqs 7.2 to 7.4. As an alternative approach, the solution may also be conveniently obtained using the cross-sectional properties of the transformed section. For example, for the cross-section of Fig. 7.4, the transformed cross-section in equivalent areas of concrete for the shortterm analysis is shown in Fig. 7.5. The cross-sectional rigidities of the transformed section deﬁned in Eqs 7.15 can be re-calculated as: RA,0 = A0 Ec,0

(7.19a)

RB,0 = B0 Ec,0

(7.19b)

RI,0 = I0 Ec,0

(7.19c) (ns(1),0 −1)As(1) (ns(2),0 −1)As(2) x yn,0 np(1),0 Ap(1) np(2),0 Ap(2)

if bonded

ns(3),0 As(3) y

Figure 7.5 Transformed cracked section with bonded reinforcement (transformed into equivalent areas of concrete).

Cracked sections 271 where A0 is the area of the transformed cracked concrete section, and B0 and I0 are the ﬁrst and second moments of the transformed area about the reference x-axis at ﬁrst loading. Substituting Eqs 7.19 into Eq. 7.18e, the matrix F0 becomes: F0 =

I0 −B0 Ec,0 (A0 I0 − B20 ) −B0 A0 1

(7.20)

Example 7.1 Assuming that the concrete can carry no tension, the position of the neutral axis and the stress and strain distributions immediately after ﬁrst loading are to be calculated on the reinforced concrete cross-section shown in Fig. 7.6 for each of the following load cases: (1) Ne,0 = 0 and Me,0 = 300 kNm; (2) Ne,0 = −1000 kN and Me,0 = 300 kNm. Both the concrete and the reinforcement are assumed to be linear-elastic with Ec,0 = 25 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = 8. 1000 100 322

Me,0

x 530

Ne,0

y As = 4000 mm2

70 400

Figure 7.6 Reinforced concrete cross-section for Example 7.1

Load case 1: Ne,0 = 0 and Me,0 = Mi,0 = 300 kNm Initially, it is assumed that the neutral axis is located in the 400 mm wide web of the cross-section. From Eq. 7.8: RA,s = As Es = 4000 × 200,000 = 800 × 106 N RB,s = ys As Es = (630 − 322) × 4000 × 200,000 = 246.4 × 109 Nmm RI,s = ys2 As Es = (630 − 322)2 × 4000 × 200,000 = 75.89 × 1012 Nmm2

272 Cracked sections With Ne,0 = Ni,0 = 0, Eq. 7.10 becomes: Ne,0 =

Ec,0 (εr,0 + yκ0 )dA + RA,s εr,0 + RB,s κ0 = 0 Ac

Dividing by κ 0 and remembering that yr,0 = −εr,0 /κ 0 gives: Ec,0 (−yn,0 + y)dA − RA,s yn,0 + RB,s = 0 Ac

which can be used to obtain a parabolic expressions in yn,0 : y=−222

y=y n,0

25,000(−yn,0 + y) × 1000 dy + y=−322

25,000(−yn,0 + y) × 400 dy

y=−222

− 800 × 106 yn,0 + 246.4 × 109 = 0 −222 yn,0 + 10 × 106 (−yn,0 y + 0.5y2 ) 25 × 106 (−yn,0 y + 0.5y2 ) −322

−222

− 800 × 106 yn,0 + 246.4 × 109 = 0 2 2 + 5yn,0 5550yn,0 + 616,100 − 8050yn,0 − 1,296,000 − 10yn,0

− 2220yn,0 − 246,400 − 800yn,0 + 246,400 = 0 2 + 1104yn,0 + 136,000 = 0 yn,0

Solving this quadratic equation gives yn,0 = −141.3 mm. Therefore the depth of the neutral axis below the top surface is dn = dref + yn,0 = 322 − 141.3 = 180.7 mm and this conﬁrms the earlier assumption that the neutral axis is located in the 400 mm wide web of the section. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 1000 × 100 + 400 × 80.7 = 132,300 mm2 ; Bc = 1000 × 100 × (50 − 322) + 400 × 80.7 × (140.35 − 322) = −33.06 × 106 mm3 ; Ic =

1000 × 1003 400 × 80.73 + 1000 × 100 × (50 − 322)2 + 12 12 + 400 × 80.7 × (140.35 − 322)2 = 8564 × 106 mm4 .

The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s = 132,300 × 25,000 + 800 × 106 = 4107 × 106 N;

Cracked sections 273 RB,0 =Bc Ec,0 +RB,s =−33.06×106 ×25,000+246.4×109 = −580.2×109 Nmm; RI,0 = Ic Ec,0 +RI,s = 8564×106 ×25,000+75.89×1012 = 290.0×1012 Nmm2 .

From Eq. 7.18e: F0 =

1 RA,0 RI,0 −R2B,0

339.4×10−12 679.1×10−15 RI,0 −RB,0 = −RB,0 RA,0 679.1×10−15 4.807 ×10−15

and the strain vector is obtained from Eq. 7.17: 0 339.4×10−12 679.1×10−15 ε0 = F0 re,0 = 300×106 679.1×10−15 4.807 ×10−15 203.7×10−6 = 1.442×10−6 mm−1 From Eq. 7.1, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: ε0(top) = εr,0 − 322 × κ0 = (203.7 − 322 × 1.442) × 10−6 = −260.6 × 10−6 ε0(btm) = εr,0 + 378 × κ0 = (203.7 + 378 × 1.442) × 10−6 = +748.8 × 10−6 The top ﬁbre stress in the concrete and the stress in the reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 25,000×(−260.6×10−6 ) = −6.52 MPa σs,0 =Es (εr,0 +ys κ0 )=200×103 ×(203.7+308×1.442)×10−6 =+129.6 MPa

The results are plotted in Fig. 7.7a. Load case 2: Ne,0 = −1000 kN and Me,0 = 300 kN.m As for load case 1, RA,s = 800×106 N, RB,s = 246.4×109 Nmm, RI,s = 75.89× 1012 Nmm2 , and it is clear that for this load case the depth of the neutral axis is greater than that for load case 1, i.e. yn,0 > −141.3 mm. In this reinforced concrete section, Eq. 7.13 reduces to: y=−y y=−222 1 1 n,0 25,000×1000×(−yn,0 +y)y dy+ 25,000×400×(−yn,0 +y)y dy−246.4×109 yn,0 +75.89×1012 Me,0 y=−322 y=−222 = y=y y=−222 Ne,0 1 1 n,0 25,000×1000×(−yn,0 +y) dy+ 25,000×400×(−yn,0 +y) dy−800×106 yn,0 +246.4×109 y=−322

y=−222

25×106 (−0.5yn,0 y2 +0.3y ˙ 3 )−222 + 10×106 (−0.5yn,0 y2 +0.3y ˙ 3 )yn,0 −246.4×109 yn,0 +75.89×1012 −322 −222 = −222 yn,0 25×106 (−yn,0 y+0.5y2 ) + 10×106 (−yn,0 y+0.5y2 )−222 −800×106 yr,0 +246.4×109 −322 =

3 +680.0×103 y 6 −1.66˙ yn,0 n,0 +299.4×10 2 −5520y 3 −5yn,0 n,0 −680.0×10

= −300 mm

274 Cracked sections Solving this cubic equation (either directly or by trial) gives yn,0 = 85.5 mm. Therefore, the depth of the neutral axis below the top surface is dn = dref +yn,0 = 407.5 mm. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 1000 × 100 + 400 × 307.5 = 223,000 mm2 Bc = 1000 × 100 × (50 − 322) + 400 × 307.5 × (253.8 − 322) = −35.59 × 106 mm3 Ic =

1000 × 1003 400 × 307.53 + 1000 × 100 × (50 − 322)2 + 12 12 + 400 × 307.5 × (253.8 − 322)2 = 9024 × 106 mm4

The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s = 223,000 × 25,000 + 800 × 106 = 6375 × 106 N RB,0 = Bc Ec,0 + RB,s = −35.59 × 106 × 25,000 + 246.4 × 109 = −643.5 × 109 Nmm RI,0 = Ic Ec,0 + RI,s = 9024 × 106 × 25,000 + 75.89 × 1012 = 301.5 × 1012 Nmm2 From Eq. 7.18e: F0 =

1 RA,0 RI,0 −R2B,0

RI,0 −RB,0 199.9×10−12 426.7 ×10−15 = −RB,0 RA,0 426.7 ×10−15 4.228×10−15

and the strain vector is obtained from Eq. 7.17:

199.9 × 10−12 426.7 × 10−15 ε0 = F0 re,0 = 426.7 × 10−15 4.228 × 10−15

−71.9 × 10−6 = 0.842 × 10−6 mm−1

−1000 × 103 300 × 106

From Eq. 7.1, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: ε0(top) = εr,0 −322×κ0 = (−71.9−322×0.842)×10−6 = −343.0×10−6 ε0(btm) = εr,0 +378×κ0 = (−71.9+378×0.842)×10−6 = +246.4×10−6

Cracked sections 275 1000 −6.52

−260.6 100 180.7 Neutral axis

+648.0

129.6

+748.8 Strain × 10−6 Stress (MPa)

Cross-section

(a) Load case 1: Ne,0 = 0 and Me,0 = 300 kN.m.

1000 −343.0

−8.57

100 407.5 Neutral axis +187.3

Cross-section

+246.4 Strain × 10−6

37.5

Stress (MPa)

(a) Load case 2: Ne,0 = −1000 kN and Me,0 = 300 kN.m.

Figure 7.7 Initial stress and strain distributions in Example 7.1.

The top ﬁbre stress in the concrete and the stress in the reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 25,000 × (−343.0 × 10−6 ) = −8.57 MPa σs,0 = Es (εr,0 + ys κ0 ) = 200 × 103 × (−71.9 + 308 × 0.842) × 10−6 = +37.5 MPa The results are plotted in Fig. 7.7b.

Example 7.2 The depth of the concrete compression zone dn and the short-term stress and strain distributions are to be calculated on the partially-prestressed concrete beam cross-section shown in Fig. 7.8a, when Me,0 = 400 kNm (and Ne,0 = 0). The section contains two layers of non-prestressed reinforcement as shown (each with Es = 2 × 105 MPa) and one layer of bonded prestressing steel (Ep = 2 × 105 MPa). The prestressing force before transfer is Pp,init = 900 kN = 3.5 MPa (i.e. σp,init = 1200 MPa). The tensile strength of the concrete is fct.f and the elastic modulus is Ec,0 = 30,000 MPa.

276 Cracked sections From Eq. 7.8: RA,s = (As(1) +As(2) )Es = (500+1000)×200,000 = 300×106 N RB,s = (ys(1) As(1) +ys(2) As(2) )Es = (−250×500+400×1000)×200,000 = 55.0×109 Nmm 2 2 RI,s = (ys(1) As(1) +ys(2) As(2) )Es = ((−250)2 ×500+4002 ×1000)×200,000

= 38.25×1012 Nmm2 RA,p = Ap Ep = 750×200,000 = 150×106 N RB,p = yp Ap Ep = 275×750×200,000 = 41.25×109 Nmm RI,p = yp2 Ap Ep = (275)2 ×750×200,000 = 11.34×1012 Nmm2 The strain in the prestressing steel caused by Pp,init before transfer is given by Eq. 7.5: εp(i),init =

900 × 103 = 6000 × 10−6 750 × 2 × 105

and the vector of actions due to initial prestress is given by Eq. 7.18d:

750 × 200,000 × 0.006 900 × 103 N fp,init = = 275 × 750 × 200,000 × 0.006 247.5 × 106 Nmm If it is initially assumed that the section is uncracked, an analysis using the procedure outlined in Section 5.3 indicates that the tensile strength of the concrete has been exceeded in the bottom ﬁbres of the cross-section. With the reference axis selected at dref = 300 mm below the top of the section, the depth of the neutral axis below the reference axis yn,0 is determined from Eq. 7.13. The left hand side of Eq. 7.13 is ﬁrst calculated: mp 0

Me,0 −

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

= (Ap(i) Ep(i) εp(i),inst )

400×106 −247.5×106 = −169.4˙ mm 0−900×103

i=1

and therefore: y=y 1 n,0

−169.4 =

30,000 × 200 × (−yn,0 + y)y dy − (55.0 + 41.25) × 109 yn,0 + (38.25 + 11.34) × 1012

y=−300 y=y 1 n,0

30,000 × 200 × (−yn,0 + y)dy − (300 + 150) × 106 yn,0 + (55.0 + 41.25) × 109

y=−300

−169.4 =

6.0 × 106 (−0.5yn,0 y2 + 0.3y ˙ 3 )yn,0 − 96.25 × 109 yn,0 + 49.59 × 1012 y−300 6.0 × 106 (−yn,0 y + 0.5y2 ) n,0 − 450 × 106 yn,0 + 96.25 × 109 −300

−169.4 =

3 + 173,750y 6 −yn,0 n,0 + 103.6 × 10 2 −3yn,0 − 2250yn,0 − 173,750

Cracked sections 277 Solving gives yn,0 = 208.1 mm. Therefore the depth of the neutral axis below the top surface is dn = dref + yn,0 = 508.1 mm. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 508.1×200−500 = 101,100 mm2 Bc = 508.1×200×(254.05−300)−500×(50−300) = −4.55×106 mm3 Ic =

200×508.13 +200×508.1×(254.05−300)2 −500×(50−300)2 12

= 2370×109 mm4 The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s + RA,p = 101,120 × 30,000 + 300 × 106 + 150 × 106 = 3484 × 106 N RB,0 = Bc Ec,0 + RB,s + RB,p = −4.55 × 106 × 30,000 + 55.0 × 109 + 41.25 × 109 = −40.24 × 109 Nmm RI,0 = Ic Ec,0 + RI,s + RI,p = 2370 × 106 × 30,000 + 38.25 × 1012 + 11.34 × 1012 = 120.7 × 1012 Nmm2 From Eq. 7.18e: F0 =

1

RI,0 −RB,0

RA,0 RI,0 −R2B,0 −RB,0 RA,0

=

288.1×10−12 96.06×10−15

96.06×10−15 8.317 ×10−15

and the strain vector is obtained from Eq. 7.17:

288.1 × 10−12 96.06 × 10−15 × ε0 = F0 re,0 − fp,init = 96.06 × 10−15 8.317 × 10−15

−244.6 × 10−6 0 − 900 × 103 = × 400 × 106 − 247.5 × 106 1.182 × 10−6 mm−1 From Eq. 7.1, the top (y = −300 mm) and bottom (y = +450 mm) ﬁbre strains are: ε0(top) = εr,0 − 300 × κ0 = (−244.6 − 300 × 1.182) × 10−6 = −599.1 × 10−6 ε0(btm) = εr,0 + 450 × κ0 = (−244.6 + 450 × 1.182) × 10−6 = +287.3 × 10−6

278 Cracked sections The distribution of strains is shown in Fig. 7.8b. 50

200

As(1) = 500 mm2

−599

−18.0 −108.1

dref = 300

Me,0 = 400 kN.m

575 700

508.1

x Neutral axis

Ap = 750 mm2

1216 Pp,init = 900 kN 45.6

As(2) = 1000 mm2 287

50 (a) Section

(b) Strain (× 10−6)

(c) Stress (MPa)

Figure 7.8 Cross-sectional details and stress and strain distributions for Example 7.2 (all dimensions in mm).

The top ﬁbre stress in the concrete and the stress in the non-prestressed reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 30,000 × (−599.1 × 10−6 ) = −18.0 MPa σs(1),0 = Es (εr,0 + ys(1) κ0 ) = 200 × 103 × (−244.6 − 250 × 1.182) × 10−6 = −108.1 MPa σs(2),0 = Es (εr,0 + ys(2) κ0 ) = 200 × 103 × (−244.6 + 400 × 1.182) × 10−6 = +45.6 MPa and the stress in the prestressing steel is given by: σp,0 = Ep εr,0 + yp κ0 + εp,init = 200 × 103 × (−244.6 + 275 × 1.182 + 6000) × 10−6 = 1216 MPa The stresses are plotted in Fig. 7.8c. 7.2.2 Axial force and biaxial bending The short-term analysis of an uncracked cross-section subjected to axial force and biaxial bending was presented in Section 6.2. The procedure is readily extended to cracked sections where the extent of cracking is evaluated based on a trial and error procedure depicted in Fig. 7.9 and described below. In the ﬁrst iteration, all concrete is initially assumed to be uncracked (Fig. 7.9a) and the analysis is identical to that described in Section 6.2. If the maximum tensile

Cracked sections 279

x

x

y

x

y

Neutral axis

Neutral axis

e

e (a) Iteration 1

(b) Iteration 2

y

Neutral axis

e (c) Iteration 3

Figure 7.9 Iterative procedure for cracked sections under axial force and biaxial bending.

stress in the concrete exceeds the tensile strength of the concrete, cracking is deemed to have occurred. In this case, the area of concrete in tension identiﬁed after the ﬁrst iteration is assumed to be cracked and to no longer contribute to the stiffness of the cross-section. This occurs, for example, in the bottom left hand corner of the cross-section shown in Fig. 7.9a, where the triangular part of the concrete section on the tensile side of the neutral axis is identiﬁed to have cracked. For the second iteration, the solution procedure remains unchanged except that the contribution of the concrete to the cross-sectional rigidities changes, with the cracked area of concrete identiﬁed in the ﬁrst iteration (shown as the unshaded region in Fig. 7.9b) now not included in the calculation of the concrete section properties (Ac , Bxc , Byc , Ixc , Iyc , Ixyc ). After the second iteration, the revised neutral axis location is determined and a new area of cracked concrete is calculated. This procedure is continued in successive iterations (Fig. 7.9c) until the differences in the calculated cross-sectional rigidities between successive iterations are negligible. From a numerical viewpoint, convergence is usually assumed to have occurred when the variations of the values of the variables deﬁning the strain diagram (i.e. ε r , κ x and κ y ) in consecutive iterations are negligible.

7.3 Time-dependent analysis (AEMM) In the analyses presented here, the fully-cracked cross-sectional area (i.e. the size of the uncracked concrete compressive zone) is assumed to remain constant with time. This assumption is not correct since creep causes a gradual change of the position of the neutral axis under sustained loads. However, as discussed in Section 7.1, the assumption greatly simpliﬁes the analysis and will usually result in relatively little error in the calculated deformations. 7.3.1 Axial force and uniaxial bending With the depth of the concrete compression zone dn assumed to remain constant with time, the time analysis of a fully-cracked cross-section using the AEMM is essentially the same as that outlined in Section 5.4.

280 Cracked sections

ds(2)

ds(1)

etop,0

etop,k As(1) As(2)

dn

x

dref

Me,k

k0 Ne,k kk

dp(1)

Ap(1) Ap(2) As(3)

dp(2) ds(3) (a) Cross-section

(b) Strain

Figure 7.10 Fully-cracked cross-section – time analysis (AEMM).

The fully-cracked cross-section shown in Fig. 7.10a is subjected to a sustained external bending moment Me,0 and axial force Ne,0 . Both the short-term and time-dependent strain distributions are shown in Fig. 7.10b. For the time analysis, the steel reinforcement and prestressing tendons (if any) are assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationship for the concrete at τ k is that given by Eq. 4.45. Therefore: σc,k = Ee,k εk − εsh,k + Fe,0 σc,0 for y ≤ yn,0 and σc,k = 0 for y > yn,0 (7.21a) σs(i),k = Es(i) εk

(7.21b)

σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(7.21c)

where Ee,k , Fe,0 and ε p.rel(i),k are as deﬁned previously (and given in Eqs 4.35, 4.46 and 5.23a). At time τ k , the internal axial force Ni,k and moment Mi,k on the cross-section are given in Eqs 5.29 and 5.31 and the axial rigidity and the stiffness related to the ﬁrst and second moments of area (RA,k , RB,k , and RI,k , respectively) are given by Eqs 5.30 and 5.32. The equilibrium equations are expressed in Eq. 5.34 and solving using Eq. 5.39 gives the strain vector at time τ k . The stresses in the concrete, steel reinforcement and tendons at time τ k are then calculated from Eqs 5.41a, b and c, respectively.

Example 7.3 The change of stress and strain with time on the cracked cross-section of Example 7.1 (Fig. 7.6) is to be calculated using AEMM. Each of the loading cases considered in Example 7.1 is to be examined here. The relevant material properties for the time period in question are: Ec,0 = 25 GPa; Es = 200 GPa; ϕ(τk , τ0 ) = 3.0; χ (τk , τ0 ) = 0.65; εsh (τk ) = −500 × 10−6 and the steel reinforcement is assumed to be linear elastic. To illustrate the effects of creep, the case when εsh (τk ) = 0 is also to be considered for load case 1.

Cracked sections 281 Load case 1a: Ne,k = 0; Me,k = Mi,k = 300 kNm and εsh (τk ) = −500 × 10−6 From load case 1 in Example 7.1, dn = 180.7 mm; εr,0 = 203.7 × 10−6 ; κ0 = 1.442 × 10−6 mm−1 ; and the shape of the cracked cross-section and the initial stress and strain distributions are illustrated in Fig. 7.7a. From Eqs 4.35 and 4.46: Ee,k =

Ec,0 25,000 = = 8475 MPa 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 3.0

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 3.0 × (0.65 − 1.0) = −0.356 Fe,0 = = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 3.0 and as calculated in Example 7.1, the properties of the concrete part of the cross-section with respect to the reference axis are Ac = 132,300 mm2 , Bc = −33.06 × 106 mm3 and Ic = 8564 × 106 mm4 and the rigidities of the steel reinforcement are RA,s = 800 × 106 N, RB,s = 246.4 × 109 Nmm and RI,s = 75.89 × 1012 Nmm2 . The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −518.3 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +140.4 × 106 Nmm The cross-sectional rigidities RA,k , RB,k and RI,k are obtained from Eqs 5.30 and 5.32: RA,k = Ac Ee,k + RA,s = 132,300 × 8475 + 800 × 106 = 1921 × 106 N Ee,k + RB,s = −33.06 × 106 × 8475 + 246.4 × 109 RB,k = Bc = −33.78 × 109 Nmm Ee,k + RI,s = 8564 × 106 × 8475 + 75.89 × 1012 RI,k = Ic = 148.5 × 1012 Nmm2 From Eq. 5.40: Fk =

1 RA,k RI,k −R2B,k

RI,k −RB,k 522.7 ×10−12 118.9×10−15 = −RB,k RA,k 118.9×10−15 6.761×10−15

and from Eqs 5.36 and 5.37: fcr,k = Fe,0

Nc,0 Mc,0

−518.1 × 103 = −0.356 × +145.4 × 106

+184.5 × 103 = −49.96 × 106

282 Cracked sections

Ac 132,300 fsh,k = Ee,k εsh,k = × 8475 × (−500 × 10−6 ) Bc −33.06 × 106

−560.6 × 103 = +140.1 × 106 For this reinforced concrete cross-section, the strain vector is obtained from Eq. 5.39: εk = Fk re,k − fcr,k + fsh,k 522.7 × 10−12 118.9 × 10−15 (0 − 184.5 − 560.6) × 103 = 118.9 × 10−15 6.761 × 10−15 (300 + 49.96 + 140.1) × 106

−331.0 × 10−6 = 3.225 × 10−6 mm−1

From Eq. 5.20, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: εk(top) = εr,k −322×κk = (−331.0−322×3.225)×10−6 = −1370×10−6 εk(btm) = εr,k +378×κk = (−331.0+378×3.225)×10−6 = +888×10−6 The concrete stresses at time τk at the top ﬁbre (y = −322 mm) and at the bottom of the compressive concrete, at yn,0 = −141.3 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−1370 + 500) × 10−6 − 0.356 × −6.52 = −5.05 MPa At yn,0 = −141.3 mm: σc,k = 8475 × (−331.0 − 141.3 × 3.225 + 500) × 10−6 − 0.356 × 0 = −2.43 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−331.0 + 308 × 3.225) × 10−6 = +132.5 MPa The results are plotted in Fig. 7.11a. Load case 1b: Ne,k = 0; Me,k = 300 kNm and εsh (τk ) = 0 The only difference from load case 1a, is that the shrinkage vector is now nil, that is, fsh,k = 0, and from Eq. 5.39, the strain vector is now: εk = Fk re,k − fcr,k + fsh,k

Cracked sections 283

522.7 × 10−12 118.9 × 10−15 (0 − 184.5 + 0) × 103 εk = 118.9 × 10−15 6.761 × 10−15 (300 + 49.96 + 0) × 106

−54.8 × 10−6 = 2.344 × 10−6 mm−1

The top and bottom ﬁbre strains are: εk(top) = εr,k − 322 × κk = (−58.8 − 322 × 2.344) × 10−6 = −810 × 10−6 εk(btm) = εr,k + 378 × κk = (−58.8 + 378 × 2.344) × 10−6 = +831 × 10−6 The concrete stresses at time τ k at the top ﬁbre and at the bottom of the compressive concrete, at yn,0 = −141.3 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−810) × 10−6 − 0.356 × −6.52 = −4.54 MPa At yn,0 = −141.3 mm: σc,k = 8475 × (−58.8 − 141.3 × 2.344) × 10−6 − 0.356 × 0 = −3.27 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−58.8 + 308 × 2.344) × 10−6 = +133.5 MPa The results are plotted in Fig. 7.11b. The effects of shrinkage acting alone are obtained by subtracting the strains and stresses calculated for load case 1b from those for load case 1a and the results are plotted in Fig. 7.11c. Load case 2: Ne,0 = −1000 kN, Me,0 = 300 kNm and εsh (τk ) = −500 × 10−6 From load case 2 in Example 7.1, dn = 407.5 mm; εr,0 = −71.9 × 10−6 ; κ0 = 0.842 × 10−6 mm−1 and the initial stress and strain distributions are illustrated in Fig. 7.7b. As for load case 1: Ee,k = 8475 MPa and Fe,0 = −0.356. As calculated in Example 7.1, the properties of the concrete part of the cross-section with respect to the reference axis are Ac = 223,000 mm2 , Bc = −35.59 × 106 mm3 and Ic = 9024 × 106 mm4 and the rigidities of the steel reinforcement are RA,s = 800 × 106 N, RB,s = 246.4 × 109 Nmm and RI,s = 75.89 × 1012 Nmm2 . The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −1150 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +253.9 × 106 Nmm

284 Cracked sections The cross-sectional rigidities RA,k , RB,k and RI,k are obtained from Eqs 5.30 and 5.32: RA,k = Ac Ee,k + RA,s = 223,000 × 8475 + 800 × 106 = 2690 × 106 N Ee,k + RB,s = −35.59 × 106 × 8475 + 246.4 × 109 RB,k = Bc = −55.23 × 109 Nmm Ee,k + RI,s = 9024 × 106 × 8475 + 75.89 × 1012 RI,k = Ic = 152.4 × 1012 Nmm2 From Eq. 5.40: Fk =

1 RA,k RI,k − R2B,k

RI,k −RB,k 374.5 × 10−12 135.7 × 10−15 = −RB,k RA,k 135.7 × 10−15 6.611 × 10−15

and from Eqs 5.36 and 5.37:

Nc,0 −1150 × 103 +409.3 × 103 Fe,0 = −0.356 × = fcr,k = Mc,0 +253.9 × 106 −90.36 × 106

223,000 Ac fsh,k = Ee,k εsh,k = × 8475 × −500 × 10−6 Bc −35.59 × 106

−945.0 × 103 = +150.8 × 106 The strain vector is obtained from Eq. 5.39: εk = Fk re,k − fcr,k + fsh,k

(−1000 − 409.3 − 945.0) × 103 374.5 × 10−12 135.7 × 10−15 = 135.7 × 10−15 6.611 × 10−15 (300 + 90.36 + 150.8) × 106

−808.3 × 10−6 = 3.258 × 10−6 mm−1 The top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are therefore: εk(top) = εr,k −322×κk = (−808.3−322×3.258)×10−6 = −1857 ×10−6 εk(btm) = εr,k +378×κk = (−808.3+378×3.258)×10−6 = +423×10−6 The concrete stresses at time τk at the top ﬁbre (y=−322 mm) and at the bottom of the compressive concrete, at yn,0 = +85.5 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−1857 + 500) × 10−6 − 0.356 × −8.57 = −8.45 MPa

Cracked sections 285 At yn,0 = +80.5 mm: σc,k = 8475 × (−808.3 + 85.5 × 3.258 + 500) × 10−6 − 0.356 × 0 = −0.39 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−808.3 + 308 × 3.258) × 10−6 = +39.0 MPa The results are plotted in Fig. 7.11d. −1370

−6.52 −5.05

−261

t0

−810

−261

−6.52 −4.54 t0

−2.43

−3.27

tk

tk

+129.6 at t0

+129.6 at t0 +132.5 at tk

+749 +888 Strain × 10−6

Strain × 10−6

Stress (MPa)

−8.57 −8.45

−343

−1857

−0.51

Stress (MPa)

(b) Load case 1b (creep only)

(a) Load case 1a (creep + shrinkage) −560

+133.5 at tk

+749 +831

t0

+0.84 tk

tk

0.39 +37.5 at t0 +57 Strain × 10−6

−1.0 at tk Stress (MPa)

(c) Load case 1c (shrinkage only)

+246 +423 Strain × 10−6

+39.0 at tk Stress (MPa)

(d) Load case 2 (creep + shrinkage)

Figure 7.11 Stress and strain distributions for Example 7.3.

Example 7.4 The change of stress and strain with time on the cracked partially-prestressed cross-section of Example 7.2 (Fig. 7.8) is to be calculated using AEMM. The actions on the section are assumed to be constant throughout the time period under consideration (i.e. τ0 to τk ) and equal to Ne,k = 0; Me,k = 400 kN.m. The relevant material properties: Ec,0 = 30 GPa; Es = Ep = 200 GPa; ϕ(τk , τ0 ) = 2.5; χ(τk , τ0 ) = 0.65; εsh (τk ) = −400 × 10−6 ; ϕ(τk , σp(i),init ) = 0.02 and the steel reinforcement is assumed to be linear elastic. From Example 7.2: dn = 508.1 mm, εr,0 = −244.6 × 10−6 , κ0 = 1.182 × 10−6 mm−1 , Ac = 101,100 mm2 , Bc = −4.55 × 106 mm3 , Ic = 2370 × 106 mm4

286 Cracked sections and the rigidities of the steel reinforcement and tendons are RA,s = 300 × 106 N, RB,s = 55.0 × 109 Nmm, RI,s = 38.25 × 1012 Nmm2 , RA,p = 150 × 106 N, RB,p = 41.25 × 109 Nmm and RI,p = 11.34 × 1012 Nmm2 . From Eqs 4.35 and 4.46: Ee,k =

30,000 = 11,430 MPa 1 + 0.65 × 2.5

and 2.5 × (0.65 − 1.0) Fe,0 = = −0.333 1.0 + 0.65 × 2.5 The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −903.2 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +117.4 × 106 N.mm The cross-sectional rigidities RA,k , RB,k and RI,k are: RA,k = Ac Ee,k + RA,s + RA,p = 101,100 × 11,430 + 300 × 106 + 150 × 106 = 1606 × 106 N Ee,k + RB,s + RB,p = −4.55 × 106 × 11,430 + 55.0 × 109 RB,k = Bc + 41.25 × 109 = 44.24 × 109 Nmm Ee,k + RI,s + RI,p = 2370 × 106 × 11,430 + 38.25 × 1012 RI,k = Ic + 11.34 × 1012 = 76.68 × 1012 Nmm2 and from Eq. 5.40: Fk =

1 RA,k RI,k −R2B,k

RI,k −RB,k 632.7 ×10−12 −365.1×10−15 = −RB,k RA,k −365.1×10−15 13.25×10−15

From Eqs 5.36 to 5.38:

Nc,0 −903.2 × 103 +301.1 × 103 ˙ fcr,k = Fe,0 = −0.333 × = Mc,0 +117.4 × 106 −39.13 × 106

Ac 101,100 fsh,k = Ee,k εsh,k = × 11,430 × −400 × 10−6 Bc −4.55 × 106 −462.2 × 103 = +20.80 × 106

Cracked sections 287 mp

Ap(i) Ep(i) 900 × 103 fp,init = ε = (from Example 7.2) yp(i) Ap(i) Ep(i) p(i),init 247.5 × 106 i=1

18 × 103 fp.rel,k = fp.init ϕp (τk , σp(i),init ) = 4.95 × 106 The strain vector is obtained from Eq. 5.39: εk = Fk re,k −fcr,k +fsh,k −fp,init +fp.rel,k

632.7×10−12 −365.1×10−15 εk = × −365.1×10−15 13.25×10−15

−1120×10−6 (0−301.1−462.2−900+18)×103 = (400+39.13+20.80−247.5+4.95)×106 3.481×10−6 mm−1 The top (y = −300 mm) and bottom (y = +450 mm) ﬁbre strains are: εk(top) = εr,k − 300 × κk = (−1120 − 300 × 3.481) × 10−6 = −2165 × 10−6 εk(btm) = εr,k + 450 × κk = (−1120 + 450 × 3.481) × 10−6 = +446.2 × 10−6 The concrete stresses at time τk at the top ﬁbre (y = −300 mm) and at the bottom of the compressive concrete, at yn,0 = 208.1 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 11,430 × (−2165 + 400) × 10−6 − 0.333 × −18.0 = −14.2 MPa At yn,0 = +208.1 mm: σc,k = 11,430 × (−1120 + 208.1 × 3.481 + 400) × 10−6 − 0.333˙ × 0 = +0.05 MPa The stress in the non-prestressed reinforcement are (Eq. 7.21b): σs(1),0 = Es (εr,0 + ys(1) κ0 ) = 200 × 103 × (−1120 − 250 × 3.481) × 10−6 = −398 MPa σs(2),0 = Es (εr,0 + ys(2) κ0 ) = 200 × 103 × (−1120 + 400 × 3.481) × 10−6 = +54.4 MPa and the stress in the prestressing steel is given by (Eq. 7.21c): σp,0 = Ep εr,0 + yp κ0 + εp.init + εp.rel,k = 200 × 103 × (−1120 + 275 × 3.481 + 6000 − 120) × 10−6 = +1143 MPa

288 Cracked sections The results are plotted in Fig. 7.12. 200 −2165

−599 tk

dref = 300

−18.0 −14.2 t0

508.1 750

−108 at t0 (−398 at tk)

t0

tk x

Me,k = 400 kN.m 0 +0.05

Pp,init = 900 kN

+1216 at t0 (+1143 at tk) +45.6 at t0 (+54.4 at tk)

287 446

Figure 7.12 Initial and time-dependent strain and stress distributions for Example 7.4 (all dimensions in mm).

7.3.2 Axial force and biaxial bending The procedure required for the time analysis of a cracked section in biaxial bending using the AEMM is identical to that for an uncracked section as presented in Section 6.3 and, for this reason, is not repeated here. The only difference is that the concrete cross-sectional properties are determined based on the shape of the cracked section identiﬁed in the instantaneous analysis. As already discussed, when modelling the timedependent behaviour of a cracked section using the AEMM, it is convenient to assume that the area of uncracked concrete does not vary with time. For most purposes, this assumption is quite reasonable and does not result in signiﬁcant error. More reﬁned computer-based methods of analysis can be used to trace the time-varying position of the neutral axis and the gradual change in shape of the cracked area of the cross-section. Such methods are discussed in the following section.

7.4 Short- and long-term analysis using the step-by-step method In some situations, time analysis of a cracked section using the AEMM may not be appropriate. For example, where the section is subjected to a complex load history, it may be necessary to use a more reﬁned analysis. A reﬁned method for the time analysis of a cracked section is described below for the cases of axial force combined with uniaxial and biaxial bending. To avoid unnecessary repetitions reference is made to the derivations presented in previous chapters. 7.4.1 Axial force and uniaxial bending 7.4.1.1 Instantaneous analysis To trace the change of position of the neutral axis and the change in shape of the cracked portion of the cross-section with time, it is convenient to subdivide the concrete

Cracked sections 289 b ds1

As1

dref x

dp1 ds2

y(i) Ap1 Ac(i)

tc(i) As2 y

Figure 7.13 Layered cross-section subjected to axial force and uniaxial bending.

into layers as shown in Fig. 7.13. With this approach, the internal actions, i.e. axial force and moment, are calculated by summing the contributions of each of the layers. Assuming that the cross-section is subdivided into mc concrete layers, and initially assuming that all concrete layers are uncracked, the contribution of the concrete component to the internal axial force Ni,0 previously introduced in Eq. 7.6 can be obtained as follows: mc

Nc,0 =

i=1 mc

=

Ac(i) σc,0 =

mc

Ac(i) Ec(i),0 (εr,0 + y(i) κ0 )

i=1 mc Ac(i) Ec(i),0 εr,0 + Bc(i) Ec(i),0 κ0

i=1

(7.22)

i=1

where Ac(i) and Bc(i) are the area and the ﬁrst moment of area of the i-th concrete layer about the x-axis; y(i) is the distance between the centroid of the i-th concrete layer and the reference axis (Fig. 7.13). This approach assumes that a constant stress is resisted by each layer calculated based on the strain measured at its centroid. Although not used here, a linearly varying stress across the thickness of each layer (t(i) ) can easily be implemented. Similarly, the contribution of the concrete to the internal moment Mi,0 is given by: Mc,0 = =

mc i=1 mc i=1

y(i) Ac(i) σc,0 =

mc

2 Ac(i) Ec(i),0 (y(i) εr,0 + y(i) κ0 )

i=1 mc Bc(i) Ec(i),0 εr,0 + Ic(i) Ec(i),0 κ0

(7.23)

i=1

where Ic(i) is the second moment of area of the i-th concrete layer about the x-axis. The concrete rigidities for the cross-section are: RA,c =

mc mc mc 2 Ac(i) Ec(i),0 ;RB,c = yc(i) Ac(i) Ec(i),0 ;RI,c = yc(i) Ac(i) Ec(i),0 i=1

i=1

i=1

(7.24a,b,c)

290 Cracked sections and the axial force and moment carried by the concrete are re-written as: Nc,0 = RA.c εr,0 + RB.c κ0

(7.25a)

Mc,0 = RB.c εr,0 + RI.c κ0

(7.25b)

In the determination of the properties of each concrete layer (Ac(i) , Bc(i) and Ic(i) ), the concrete displaced by the presence of any reinforcement or tendons in a layer is often ignored, but it is usually straightforward to include the actual concrete area rather than the gross area of the concrete layer. The number of layers (mc ) to be speciﬁed at the beginning of the analysis should be sufﬁcient to produce accurate results. A simple approach to determine mc is to compare the values for the cross-sectional ﬂexural rigidity RI,0 calculated considering the uncracked cross-section with and without layers. The number of layers is acceptable when the difference between these two values is less than 1 per cent. The governing equilibrium equations for a typical cross-section are therefore: Ni,0 = (RA,c + RA,s + RA,p )εr,0 + (RB,c + RB,s + RB,p )κ0 +

mp Ap(i) Ep(i) εp(i),init = Ne,0

(7.26a)

i=1

Mi,0 = (RB,c + RB,s + RB,p )εr,0 + (RI,c + RI,s + RI,p )κ0 mp yp(i) Ap(i) Ep(i) εp(i),init = Me,0 +

(7.26b)

i=1

where the concrete rigidities are given by Eq. 7.24 and the rigidities of the reinforcement and the tendons are deﬁned in Eqs 7.8. This system of two equations can be used to solve for the two unknowns εr,0 and κ0 . To determine the extent of cracking, the solution process is iterative. For the ﬁrst iteration all concrete layers are assumed to be uncracked, that is, each concrete layer contributes to the cross-sectional stiffness. The cross-section is analysed and the concrete stress at the centroid of each layer is determined. For the second iteration, concrete layers subjected to tension in the ﬁrst iteration in excess of the tensile strength of concrete are assumed to have cracked and are subsequently neglected, i.e. the value Ec(i),0 in a cracked layer is set to zero. At the end of each subsequent iteration the stresses are checked in the uncracked layers to identify whether any additional layers have cracked. The short-term analysis is terminated when no additional cracking is detected. More reﬁned material models could be implemented, including the effects of tension-stiffening, tension-softening or other material nonlinearities, and more efﬁcient solving strategies could be used. 7.4.1.2 Time analysis The step-by-step method (SSM) of analysis is adopted. The time discretisation associated with the method was discussed in Section 4.3.1 and the analysis of uncracked cross-sections was presented in Section 5.5, with the constitutive relationships for the concrete, reinforcement and tendons given in Eqs 4.25 and 5.44.

Cracked sections 291 The steps required for the long-term analysis of a cracked section are similar to those required for an uncracked section. The only difference in this case is that the concrete in a cracked layer is assumed to carry no tension. For the layered section of Fig. 7.13, the axial force and moment carried by the concrete to be included in the expression for the internal actions (Eqs 5.50 and 5.51) and the equilibrium equations (Eq. 5.54) can be calculated from:

Nc,j =

mc i=1

=

mc

Ac(i) σc(i),j = ⎛

mc

⎛

⎞ j−1 ⎝Ac(i) Ec(i),j ε(i),j − εsh,j + Fe,j,n σc(i),n Ac(i) ⎠

i=1

n=0

⎝Ac(i) Ec(i),j εr,j + Bc(i) Ec(i),j κj − Ac(i) Ec(i),j εsh,j +

i=1

Mc,j =

mc i=1

=

mc

j−1

⎞ Fe,j,n σc(i),n Ac(i) ⎠

n=0

y(i) Ac(i) σc(i),j = ⎛

mc

⎛

j−1

(7.27a) ⎞

⎝y(i) Ac(i) Ec(i),j ε(i)j − εsh,j + Fe,j,n σc(i),n y(i) Ac(i) ⎠

i=1

⎝Bc(i) Ec(i),j εr,j + Ic(i) Ec(i),j κj − Bc(i) Ec(i),j εsh,j +

i=1

i=0 j−1

⎞

Fe,j,n σc(i),n Bc(i) ⎠

n=0

(7.27b) where the stress history of each layer is recorded separately and the contribution of all cracked layers is zero. As for the instantaneous analysis, an iterative procedure is adopted at each time step. During any iteration, if cracking is detected in a previously uncracked concrete layer (i.e. if the stress at the centroid of the layer exceeds the tensile strength of concrete), the contribution to the cross-sectional rigidities of the concrete in that layer is set to zero and the previous stress history for that layer is subsequently ignored. If the stress in a previously cracked layer becomes compressive, the crack is deemed to have closed and the concrete in the layer begins to contribute to the cross-sectional stiffness and, for the purposes of subsequent creep calculations, the stress history for the layer is stored from this point in time. The iterative procedure continues until the changes in the calculated strain diagram (i.e. the changes in εr,j and κj ) from one iteration to the next are sufﬁciently small. 7.4.2 Axial force and biaxial bending The geometric discretisation required for the analysis of a cross-section subjected to combined axial force and biaxial bending is shown in Fig. 7.14. The cross-section is subdivided both horizontally and vertically into smaller rectangular areas (similar to the layers introduced in the previous section for the case of uniaxial bending). In each rectangular concrete area, the stress is assumed to be constant and is calculated from the strain measured at its centroid. A linearly varying stress distribution could also be considered based on strain values calculated at each corner of the subdivision.

292 Cracked sections

x

y(i)

Ac(i) y

x(i)

Figure 7.14 Geometric discretisation of cross-section - axial force and biaxial bending.

As suggested previously, the ﬁneness of the subdivision to be used for the analysis can be determined by comparing the values of the uncracked ﬂexural rigidities RIx,k , RIy,k and RIxy,k calculated with and without the subdivisions. When the differences are less than 1 per cent, the degree of discretisation is acceptable. The solution process for cracked sections in biaxial bending is identical to that described in Section 7.4.1. In the ﬁrst iteration of the instantaneous analysis, all concrete is assumed to be uncracked. The cracked areas of concrete are identiﬁed and ignored in the next and subsequent iterations. This iterative procedure is applied at each time step, where the effects of creep from the previously stored stress history in each subdivision and the effects of shrinkage are determined. Further changes in the extent of cracking are identiﬁed at the end of each iteration, as are locations where the cracks may have closed in previously cracked regions. In this way, the timedependent changes in deformation and stresses are calculated, without the simplifying assumptions inherent in the AEMM, where a single time step is considered and the extent of cracking on the cross-section is assumed not to change with time.

7.5 References 1. Bischoff, P.H. (2001). Effects of shrinkage on tension stiffening and cracking in reinforced concrete. Canadian Journal of Civil Engineering, 28(3), 363–374. 2. Gilbert, R.I. and Wu, H.Q. (2009). Time-dependent stiffness of cracked reinforced concrete elements. ﬁb London 09, Concrete: 21st Century Superhero, June, London. 3. Scott, R.H. and Beeby, A.W. (2005). Long-term tension stiffening effects in concrete. ACI Structural Journal, 102(1): 31–39. 4. Bamforth, P.B. (2007). Early-age thermal crack control in concrete. CIRIA C660, London.

8

Members and structures

8.1 Introductory remarks The cross-sectional analyses developed in Chapters 4–7 form the basis for the prediction of the in-service deformation of concrete members and structures. Techniques for making such predictions are presented in this chapter. From the point of view of serviceability, it is important that the deﬂection and shortening of structural members remain acceptably small under normal in-service conditions. It is also important that crack widths are such that they do not detract from the appearance or durability of the structure. In Chapter 3, some guidance was given for the design of concrete structures for serviceability. The load combinations and design criteria for the serviceability limit states that are speciﬁed in some of the more well-known codes of practice were discussed. In this chapter, procedures for the prediction of structural behaviour at service loads for a variety of structural forms are discussed and illustrated. In most cases, reference is made to the relevant cross-sectional analyses described and illustrated in Chapters 4–7. Throughout this chapter the age-adjusted effective modulus method (AEMM) has been adopted for the analysis of the individual cross-sections, however, the member analyses could be carried out just as easily using any of the other methods of analysis introduced in Chapter 4 [such as the effective modulus method (EEM), step-by-step method (SSM) or rate of creep method (RCM)]. In Section 8.5, the effects of timedependent displacements on the behaviour of slender reinforced concrete columns at the strength limit state are also considered. Often the accurate prediction of structural behaviour at service loads is difﬁcult, particularly for many-fold indeterminate structures, but useful approximations are available to simplify many of the calculations. In the analyses presented here, approximations and simplifying assumptions are introduced from time to time to reduce the computational effort. In design, a thorough understanding of the nature and implications of these assumptions is essential if a realistic and practical interpretation of the ﬁnal results is to be made. As with all aspects of structural analysis and design, sound engineering judgment is an essential ingredient.

8.2 Deﬂection of statically determinate beams 8.2.1 Deﬂection and axial shortening of uncracked beams In Section 3.6.1, the calculation of the deﬂection and axial shortening of a member by integration of the deformations over the length of the member was discussed. If the

294 Members and structures curvature and axial strain at the centroid of the section are known at each end of a span (i.e. at cross-sections A and B in Fig. 3.1) and at mid-span (cross-section C in Fig. 3.1) and if the distributions of axial strain and curvature along the member are parabolic, the axial deformation and mid-span deﬂection of the member are given by Eqs 3.7a and b, given here and renumbered for convenience: eAB =

(εaA + 4εaC + εaB ) 6

(8.1a)

vC =

2 (κA + 10κC + κB ) 96

(8.1b)

Example 8.1 The axial shortening and mid-span deﬂection of a simply-supported, uncracked, post-tensioned concrete beam spanning 12.0 m are to be calculated, immediately after ﬁrst loading and after a period of sustained loading at time τk . An elevation of the beam is shown in Fig. 8.1, together with details of the cross-section at mid-span. The non-prestressed reinforcement is uniform along the span. The beam is post-tensioned by a single cable of parabolic proﬁle, with the depth of the tendon below the top surface of the beam (dp ) equal to 450 mm at each support and 780 mm at mid-span. The duct diameter is 70 mm. The initial tensile force in the tendon prior to transfer (at time τ0 ) is assumed to be constant along the length of the member and equal to Pp,init = 1300 kN. That is, σp,init = Pp,init /Ap = 1300 MPa at every cross-section. The prestressing duct is grouted soon after the transfer of prestress and immediately after the application of the sustained load, so that the prestressing tendon is unbonded for the short-term analysis but fully bonded to the concrete throughout the period of the time analysis. Two load cases are considered. In load case 1, the beam is subjected only to its self-weight (i.e. ws = 6.1 kN/m) plus prestress from ﬁrst loading to time τk . In load case 2, the beam carries a constant sustained uniformly distributed load of ws = 40 kN/m plus prestress from ﬁrst loading to time τk . The relevant material properties for the time period under consideration are: Ec (τ0 ) = 30,000 MPa Es = Ep = 2 × 105 MPa ϕ(τk , τ0 ) = 1.8 χ(τk , τo ) = 0.65 εsh (τk − τo ) = −400 × 10−6 and ϕp (τk , σp,init ) = 0.02 Taking the centroidal axis of the gross cross-section as the reference axis (i.e. dref = 450 mm), the initial and ﬁnal strains at the reference axis and the initial and ﬁnal curvatures are ﬁrst calculated at mid-span and at each support using the

Members and structures

295

ws 450

450

A

C

Parabolic tendon

B

6000

6000

Elevation 50

450

As(1) = 1200 mm2 450 850 780

Centroid of gross section

Agross = 254,000 mm2 Igross = 22,500 × 106 mm4 (with respect to centroidal axis)

900

Ap(1) = 1000 mm2 As(2) = 2400 mm2

Section at mid-span

Figure 8.1 Details of beam in Example 8.1 (all dimensions in mm).

cross-section analyses outlined in Sections 5.3 and 5.4. The axial deformation and deﬂection are then calculated using Eqs 8.1. For the short-term analyses, the duct is empty and the prestressing steel does not contribute to the properties of the transformed section. For the long-term analysis the duct is grouted and the prestressing steel forms part of the transformed cross-section.

Load case 1 Cross-section at mid-span The applied moment at mid-span caused by the sustained load ws = 6.1 kN/m is: Ms =

6.1 × 122 = 109.8 kNm 8

and from a cross-sectional analysis of Section 5.3, the strain at the reference axis and the curvature immediately after ﬁrst loading are εr,0 = −158 × 10−6 and κ0 = −0.411 × 10−6 mm−1 . The strain at the reference axis and the curvature at mid-span at time τk are calculated using the analysis of Section 5.4 and are equal to εr,k = −662 × 10−6 and κk = −0.641 × 10−6 mm−1 . In the time analysis, the grout was initially assumed to be unloaded. Cross-section at the supports Similar calculations for the section at each support, where Ms = 0 and dp = 450 mm, give εr,0 = −160 × 10−6 ; κ0 = 0.017 × 10−6 mm−1 ; εr,k = −690 × 10−6 ; and κk = 0.163 × 10−6 mm−1 .

296 Members and structures Axial shortening and deﬂection Using Eq. 8.1a, the axial shortening of the member is: At ﬁrst loading: ei =

12,000 (−160 − 4 × 158 − 160) × 10−6 = −1.90 mm 6

At time τk : 12,000 (−690 − 4 × 662 − 690) × 10−6 = −8.06 mm 6 The initial and ﬁnal mid-span deﬂections are found using Eq. 8.1b and are: e=

At ﬁrst loading: vci =

12,0002 [0.017 + 10 × (−0.411) + 0.017] × 10−6 96

= −6.11 mm (i.e. upward camber) At time τk : vc =

12,0002 [0.163+10×(−0.641)+0.163]×10−6 = −9.13 mm 96

Load case 2 The applied moment at mid-span caused by the sustained load ws = 40.0 kN/m is Ms = 40 × 122 /8 = 720 kNm and the strain at the reference axis and the curvature immediately after ﬁrst loading and after the period of sustained loading are εr,0 = −162 × 10−6 ; κ0 = +0.392 × 10−6 mm−1 ; εr,k = −727 × 10−6 ; and κk = +1.116 × 10−6 mm−1 . The strain and curvature at each support are the same as those calculated for load case 1, since at each support the applied moment Ms in both cases is zero. That is εr,0 = −160 × 10−6 ; κ0 = 0.017 × 10−6 mm−1 ; εr,k = −690 × 10−6 ; and κk = 0.163 × 10−6 mm−1 . Axial shortening and deﬂection The axial shortening and deﬂection of the member are obtained from Eqs 8.1a and b: At ﬁrst loading: ei = vci =

12,000 (−160 − 4 × 162 − 160) × 10−6 = −1.94 mm 6 12,0002 (0.017 + 10 × 0.392 + 0.017) × 10−6 = 5.93 mm 96

At time τk : e= vc =

12,000 (−690 − 4 × 727 − 690) × 10−6 = −8.58 mm 6 12,0002 (0.163 + 10 × 1.116 + 0.163) × 10−6 = 17.23 mm 96

Members and structures

297

The stress and strain distributions on the cross-section at mid-span are shown in Fig. 8.2 for both load cases. −373

+0.13 +0.81

+26.9

tk

ss1 = 1.3 (−81.1) t0

t0

−0.641 × 10−6 mm−1 −0.411 × 10−6 mm−1 −950 Section

tk

sp = 1300 (1099)

ss2 = −64.5 (−184) −10.28 −4.61 Stress (MPa)

−343 Strain (× 10−6) (a) Load case 1 −339

−1230

−10.2 −8.52 tk

t0 +1.109 × 10−6 mm−1 tk

Section

t0

+0.392 × 10−6 mm−1

−225 Strain (× 10−6)

ss1 = −63.8 (−235)

+14.1

sp = 1300 (1202) ss2 = −1.1 (−56.1) +0.42 +2.30 Stress (MPa)

(a) Load case 2

Figure 8.2 Stress and strain on cross-section at mid-span for Example 8.1.

8.2.2 Control of deﬂection using non-prestressed reinforcement The change in curvature on a cross-section depends on the quantity and location of the bonded reinforcement. Consider the beam analysed in Example 8.1 and shown in Fig. 8.1. By increasing the area of top steel, As(1) , on the cross-section at mid-span, the rate of change of positive curvature with time would decrease. Increased amounts of top steel are particularly effective in reducing the time-dependent increase in positive curvature when the applied load is sufﬁciently high to induce signiﬁcant compressive stresses in the top ﬁbres, such as for load case 2 in Example 8.1. An increase in top steel would therefore reduce the ﬁnal downward deﬂection of the beam in Example 8.1 (load case 2). However, when the initial curvature is negative, as for load case 1, an increased amount of top steel would cause an increase in the negative curvature with time and an increase in the upward deﬂection. By increasing the area of bottom steel, As(2) , on the cross-section at mid-span, the rate of change of positive curvature with time would increase. Increased amounts of bottom steel are particularly effective in reducing the time-dependent increase in negative curvature when the applied load on a prestressed member is small and the compressive stresses in the bottom ﬁbres are relatively high, such as for load case 1 in Example 8.1. An increase in bottom steel would therefore reduce the ﬁnal upward

298 Members and structures deﬂection of the beam for load case 1. However, when the initial curvature is positive, as for load case 2, an increased amount of bottom steel would cause an increase in the positive curvature with time and an increase in the downward deﬂection. Tables 8.1 and 8.2 show the results of several time analyses of the beam shown in Fig. 8.1 subjected to different levels of applied loading. The areas of top and bottom non-prestressed reinforcement are varied to assess the effects of steel quantity and position on the ﬁnal deﬂection. The prestressing steel details, including the cable drape and prestressing force, the cross-sectional dimensions and the material properties are as given in Example 8.1. Three different values of the sustained load are considered, namely ws = 6.1, 23.8 and 40 kN/m. When ws = 6.1 kN/m (corresponding to the self-weight of the beam only), the initial concrete stress distribution at mid-span is approximately triangular with high compressive stress at the bottom of the cross-section, decreasing to zero stress near the top of the cross-section (as determined in Example 8.1 and illustrated in Fig. 8.2a). The load level ws = 23.8 kN/m corresponds to the balanced load stage where the external load is balanced by the upward uniformly distributed load exerted on the beam by the parabolic prestressing tendon. At this balanced load stage, the initial stress distribution is uniform over the depth of each section and the initial curvature on each section is very small. When the applied load ws = 40 kN/m, the initial stress distribution at midspan is again approximately triangular with high compressive stress at the top of the section decreasing to zero near the bottom of the section (as shown in Fig. 8.2b). The moment at mid-span is therefore close to the decompression moment. From the results in Table 8.1, the effect of increasing the quantity of non-prestressed bottom reinforcement, As(2) , is to increase the restraint to creep and shrinkage deformation in the bottom of the section and thereby increase the change in positive or sagging curvature with time. The increase is most pronounced when the initial concrete compressive stress at the level of the steel is high, i.e. when the sustained applied moment is low and the section is initially subjected to a negative or hogging curvature. Increasing the quantity of bottom reinforcement therefore increases the change in downward deﬂection with time. When the beam is subjected only to its self-weight (ws = 6.1 kN/m), increasing As(2) from zero to 4800 mm2 (p = As(2) /bd = 1.25%) changes the time-dependent deﬂection from −8.55 mm (upwards) to +3.77 mm (downwards). Evidently, the inclusion of additional bottom reinforcement is an excellent way of reducing or eliminating the time-dependent upward deﬂection or camber that often causes serviceability problems in prestressed concrete construction when the sustained load is relatively light. When the beam is initially subjected to the balanced load (ws = 23.8 kN/m), increasing As(2) from zero to 4800 mm2 changes the time-dependent deﬂection from +2.90 mm (downwards) to +11.36 mm (downwards). When the sustained load is sufﬁcient to decompress the bottom ﬁbres at mid-span (ws = 40.0 kN/m), increasing As(2) from zero to 4800 mm2 changes the time-dependent deﬂection from +13.38 mm (downward) to +18.32 mm (downwards). The inclusion of tensile non-prestressed reinforcement in the bottom of a prestressed beam may increase the downward deﬂection with time and may in fact cause undesirable deﬂection in some situations. From the results in Table 8.2, the inclusion of non-prestressed reinforcement in the compressive zone, As(1) , increases the restraint to creep and shrinkage deformation in the top of the section and thereby increases the change in negative or hogging curvature with time (or reduces the change in positive curvature with time). The effect

κ0 (×10−6 mm−1 ) −0.492 −0.412 −0.350 −0.011 0.027 0.057 0.429 0.429 0.429

εr,0 (×10−6 )

−175 −158 −144

−173 −165 −158

−171 −171 −171

As(2) (mm2 )

0 2400 4800

0 2400 4800

0 2400 4800

ws (kN/m)

6.1

23.8

40.0

Initial deformation of section at mid-span

6.44 6.55 6.63

0.16 0.52 1.04

−7.38 −6.06 −5.06

Initial deﬂection at mid-span (mm)

−676 −646 −628

−655 −592 −557

−632 −534 −478

0.892 1.029 1.113

0.193 0.482 0.649

−0.570 −0.115 0.143

εr,k κk (×10−6 ) (×10−6 mm−1 )

– −46.9 −36.6

– −79.9 −59.4

– −116 −84.3

σs(2),k (MPa)

Change in deformation and steel stress with time on section at mid-span

Table 8.1 Effect of varying the area of non-prestressed tensile steel As(2) (As(1) = 0)

−108 −93.2 −84.1

−180 −144 −122

−258 −199 −164

σp,k (MPa)

13.38 16.48 18.32

2.90 8.28 11.36

−8.55 −0.68 3.77

Change in mid-span deﬂection with time (mm)

−0.412 −0.410 −0.409 0.027 −0.008 −0.036 0.429 0.360 0.306

−158 −158 −158

−165 −156 −150

−171 −155 −142

0 2400 4800

0 2400 4800

0 2400 4800

6.1

23.8

40.0

6.55 5.39 4.50

0.52 −0.12 −0.62

−6.06 −6.15 −6.22

−646 −506 −428

−592 −494 −439

−534 −481 −450

1.029 0.506 0.217

0.482 0.114 −0.094

−0.115 −0.315 −0.433

– −142 −103

– −108 −80.3

– −71.1 −55.4

−46.9 −60.8 −68.3

−79.9 −89.9 −95.3

−116 −121 −125

−93.2 −101 −106

−144 −149 −152

−199 −202 −203

σs(1),k σs(2),k σp,k (MPa) (MPa) (MPa)

Change in deformation and steel stress with time on section at mid-span

κ0 εr,0 Initial deﬂection εr,k ws As(1) κk (kN/m) (mm2 ) (×10−6 ) (×10−6 mm−1 ) at mid-span (mm) (×10−6 ) (×10−6 mm−1 )

Initial deformation of section at mid-span

Table 8.2 Effect of varying the area of non-prestressed compressive steel As(1) (As(2) = 2400 mm2 )

16.5 7.59 2.67

8.27 1.70 −1.46

−0.68 −4.73 −7.08

Change in mid-span deﬂection with time (mm)

Members and structures

301

is most pronounced when the initial concrete compressive stress at the level of the top steel is high, i.e. when the sustained applied moment is high and the section is initially subjected to a positive or sagging curvature. Increasing the quantity of top reinforcement therefore decreases the change in downward deﬂection with time. When the beam is subjected only to self-weight (ws = 6.1 kN/m), increasing As(1) from zero to 4800 mm2 (p = As(1) /bd = 1.25%) changes the time-dependent deﬂection from −0.68 mm (upwards) to −7.08 mm (upwards). The inclusion of top reinforcement therefore increases the upward camber in a prestressed concrete member with time. When the beam is initially subjected to the balanced load (ws = 23.8 kN/m), increasing As(1) from zero to 4800 mm2 changes the time-dependent deﬂection from +8.27 mm (downward) to −1.46 mm (upwards). When the sustained load is sufﬁcient to decompress the bottom ﬁbres at mid-span (ws = 40.0 kN/m), increasing As(1) from zero to 4800 mm2 reduces the time-dependent deﬂection from +16.5 mm (downward) to +2.67 mm (downwards). The inclusion of non-prestressed compressive reinforcement in the top of a reinforced or prestressed beam substantially reduces the long-term downward deﬂection. The signiﬁcant reduction with time of the resultant compressive force carried by the concrete should also be noted. In Tables 8.1 and 8.2, the time-dependent changes in the bonded steel stress on the cross-section at mid-span are reported. This gradual build up of compression in the steel at each level of bonded reinforcement is balanced by an equal and opposite tensile force acting on the concrete at that level of magnitude As(i) σs(i) or Ap σp . In Table 8.2, for example, when ws = 23.8 kN/m and when As(1) = As(2) = 2400 mm2 , the concrete on the section at mid-span is subjected to three gradually increasing tensile forces (i.e. As(1) σs(1) = 259 kN, As(2) σs(2) = 216 kN and Ap σp = 149 kN). Initially the concrete was subjected to a net compressive prestressing force of 1300 kN, but this reduces by 624 kN with time. About 48 per cent of the initial compression in the concrete is shed into the bonded reinforcement with time. The loss of prestress in the tendon is only 149 kN (11.5 per cent). Clearly, a reliable picture of the time-dependent behaviour of a partially prestressed concrete beam cannot be obtained unless the restraint provided to creep and shrinkage by the non-prestressed reinforcement is adequately accounted for. It is also evident that the presence of non-prestressed reinforcement signiﬁcantly reduces the cracking moment with time and may in fact relieve the concrete of much of its initial prestress. This increases the possibility of time-dependent cracking and the effect should be included in design considerations. Although, the restraint provided by the bonded reinforcement, generally lowers the cracking moment, a judicious placement of nonprestressed reinforcement is an effective means of controlling deﬂection and can even be used to eliminate the time-dependent change in deﬂection in situations where such changes in deﬂection are undesirable. 8.2.3 Deﬂection and axial shortening of cracked beams In Chapter 3, code-oriented methods for the prediction of deﬂection in reinforced and prestressed concrete members were presented. Where more reliable predictions of deformation are needed, more reﬁned methods of analysis may be required such as those for uncracked cross-sections, outlined in Chapters 5 and 6, and for cracked crosssections, discussed in Chapter 7. These methods of analysis may be used to predict the deﬂection of cracked members.

302 Members and structures Clearly, for a cracked member, deﬂection will be underestimated if the analysis assumes every cross-section is uncracked. On the other hand, deﬂection will be overestimated, sometimes grossly overestimated, if every cross-section is assumed to be fully cracked. Tension stiffening, or the contribution of the tensile concrete to the member stiffness, ensures that the actual deﬂection of a cracked member lies somewhere between these two extremes, i.e. between the deﬂection in the uncracked condition and in the fully-cracked condition. According to Eurocode 2 (Ref. 1), to account for tension stiffening, the average curvature at a particular cracked cross-section may be taken from Eq. 3.23 (reproduced here as Eq. 8.2): κavge = ζ κ cr + (1 − ζ )κuncr

(8.2)

where ζ is the distribution coefﬁcient presented earlier as Eq. 3.24b. The most rigorous method for determining deﬂection using the cross-sectional analyses presented in Chapters 4–7 is to calculate the cracked and uncracked curvatures at frequent cross-sections along the member and then to calculate the average curvature at each section using Eq. 8.2. For this purpose the distribution coefﬁcient ζ may be taken as:

Mcr.t 2 (8.3) ζ = 1− Ms∗ where Mcr.t is the cracking moment at the time under consideration and Ms∗ is the maximum in-service moment that has been imposed on the member at, or before, the time instant at which deﬂection is being determined. With the curvature diagram thus determined, the deﬂection can be obtained by numerical integration. If the curvatures at the critical cross-sections are calculated using Eq. 8.2, the mid-span deﬂection at the time under consideration may be conveniently obtained using Eq. 8.1b.

Example 8.2 The initial and long-term deﬂections at mid-span of a 10.4 m span simplysupported reinforced concrete T-beam are to be calculated. The beam carries a constant sustained uniformly distributed service load of 22.2 kN/m (which includes self-weight) ﬁrst applied at age τ0 . Details of the cross-section and the relevant material properties are shown in Fig. 8.3. The reinforcement is uniform throughout and shrinkage is assumed to commence at τ0 . The cross-section is the same as that shown in Fig. 7.6 and analysed in Examples 7.1 and 7.3. The = 0.6 f = 3.0 MPa, ﬂexural tensile strength of the concrete is taken to be fct.f c , cracking is deemed to have so wherever the extreme ﬁbre stress exceeds fct.f occurred. The bending moment diagram for the simply-supported span is illustrated in Fig 8.4a. From a short-term analysis of the uncracked cross-section, the stress = 3.0 MPa when the applied moment in the bottom concrete ﬁbres reaches fct.f is 149.3 kNm, i.e. at points D and D’ in Fig. 8.4a, 1.514 m from each support. It is evident that, within 1.514 m from each support, the member is initially uncracked, whilst further into the span cracking occurs.

Members and structures

303

1000

f ′c = 25 MPa

100

Ec = 25,000 MPa

322

x

Es = 200,000 MPa

530

f(tk ,t0) = 3.0

y

c(tk ,t0) = 0.65

As = 4000 mm2

70

esh(tk − t0) = −500 × 10−6

400

Figure 8.3 Cross-sectional details and material properties for Example 8.2 (dimensions in mm).

Using the cross-sectional analyses of Sections 5.3 (short-term) and 5.4 (timedependent) for the uncracked portions of the span and Sections 7.2 (short-term) and 7.3 (time-dependent) for each fully-cracked cross-section, the initial and ﬁnal curvatures at any cross-section along the member may be calculated. It is noted that shrinkage causes an increase in the bottom ﬁbre tensile stress in the concrete on the uncracked cross-sections, effectively reducing the cracking moment from 149.3 kNm to 56.4 kNm with time. The extent of cracking therefore increases with time until eventually only 0.514 m at each end of the span remains uncracked. In Fig. 8.4b, the portion of the curvature diagram at time τk between points E and D on the span is approximated as a straight line. 10.4 m 1.514 m 0.514 m A 56.4 B

E

C

D

D′

149.3

300

(a) Bending moment (kNm) 1.514 m

0.521 × 10−6 0.885 × 10−6

0.318 × 10−6 0.718 × 10−6 1.442 × 10−6

2.053 × 10−6

At t0 3.237 × 10−6

At tk

(b) Curvature (mm−1) Figure 8.4 Bending moment and curvature diagrams of Example 8.2.

304 Members and structures Plots of the initial and ﬁnal curvatures are made in Fig 8.4b and a summary of the calculated curvatures at various points along the beam is made in Table 8.3. Table 8.3 Initial and ﬁnal curvatures in beam of Example 8.2 At time τ0

At time τk

Distance from support, z (mm)

Moment (kNm)

Curvature (mm−1 )

Moment (kNm)

Curvature (mm−1 )

0 0.514 1.514 − 1.514 + 3.075 5.2

0 56.4 149.3 149.3 250.0 300.0

0 0.120 × 10−6 0.318 × 10−6 0.718 × 10−6 1.202 × 10−6 1.442 × 10−6

0 56.4 149.3 149.3 250.0 300.0

0.521 × 10−6 0.885 × 10−6 2.053 × 10−6 2.053 × 10−6 2.841 × 10−6 3.237 × 10−6

The initial mid-span deﬂection of the cracked member at ﬁrst loading τ0 and the ﬁnal deﬂection at time τk calculated by numerically integrating these curvature diagrams are: (vc )cr.0 = 15.98 mm and (vc )cr.k = 38.14 mm. A close approximation of these more accurate (but considerably more tedious) calculations may be obtained using Eq. 8.1b (viz., (vc )cr.0 = 16.25 mm and (vc )cr.k = 37.64 mm). If cracking was ignored and the curvature diagrams were calculated based on the uncracked section properties, the mid-span deﬂection at times τ0 and τk would be (vc )uncr.0. = 7.19 mm and (vc )uncr.k = 28.03 mm. At time τ0 and τk , Eq. 8.3 gives: ζ0 = 1 −

149.3 300

2 = 0.752 and ζk = 1 −

56.4 300

2 = 0.965

and using the following expressions (similar to Eq. 8.2), the ﬁnal mid-span deﬂections of the cracked member accounting for tension stiffening at ﬁrst loading and at time τk are: vc.0 = ζ (vc )cr.0 + (1 − ζ )(vc )uncr.0 = 0.752 × 15.98 + (1 − 0.752) × 7.19 = 13.8 mm vc.k = ζ (vc )cr.k + (1 − ζ )(vc )uncr.k = 0.965 × 38.14 + (1 − 0.965)×28.03=37.8 mm

For most practical purposes, knowledge of the curvature at each end of a member and at mid-span at any particular time after ﬁrst loading is generally sufﬁcient to make a reliable estimate of the deﬂection of a cracked reinforced concrete member.

Members and structures

305

8.3 Statically indeterminate beams and slabs 8.3.1 Discussion In each cross-sectional analyses presented in Chapters 4–7, the internal actions were known and the changes in strain and curvature on a particular cross-section were assumed to occur without restraint from either the supports or adjacent parts of the structure. While this assumption is perfectly reasonable for statically determinate members, it may be unreasonable for continuous members. Consider a plain concrete continuous beam subjected to a uniformly distributed load that is small enough to avoid cracking. If the concrete is assumed to be homogeneous, with the same creep characteristics throughout, the effect of creep is simply to reduce the effective modulus and to increase the strains and displacements with time. There is no change in the reactions at the supports and consequently no change in the internal actions on any cross-section. However, if the creep characteristics are not uniform throughout, creep will induce reactions at the supports and cause a change in the distribution of internal actions. In practical concrete structures, the creep characteristics are rarely uniform. Different parts of a structure may have different ages and therefore different creep coefﬁcients. If part of a structure has cracked, its response to creep is different from that of the uncracked parts of the structure. In addition, the quantity of reinforcement may vary from region to region and therefore the amount of internal restraint to creep will vary accordingly. Therefore, in statically indeterminate concrete structures, creep may lead to a considerable redistribution of internal actions with time. Shrinkage also may cause signiﬁcant changes in the distribution of internal actions with time in indeterminate members. If a member is not free to shorten, shrinkage produces internal tension. Shrinkage-induced curvature on each cross-section due to the restraint provided by asymmetrically placed steel reinforcement can introduce signiﬁcant reactions at the supports and hence signiﬁcant changes in the internal actions on each cross-section. Consider the uncracked, propped cantilevers shown in Fig. 8.5. The member in Fig. 8.5a(i) contains a preponderance of reinforcement in the bottom ﬁbres and shrinkage causes a positive curvature in the singly reinforced region. If the weight of the beam and any applied loads are ignored and if the support at B is removed, shrinkage would cause the member to gradually deﬂect upwards, as indicated. With the support at B, in fact, resisting upward movement, a downward reaction RB.k gradually develops with time, as shown. The initial reaction at B caused by the load on the beam RB.0 is therefore reduced by RB.k and this leads to an increase in the negative moment at support A and a decrease in the positive moment at mid-span. Shrinkage therefore causes the time-dependent redistribution of moments shown in Fig. 8.5b(i). Note that the shrinkage-induced reactions at the built-in support at A (namely, a vertical reaction RA.k , equal and opposite to RB.k , and a moment MA.k = RB.k L) are not shown in Fig. 8.5. For the member shown in Fig. 8.5a(ii), with a preponderance of steel in the top, shrinkage causes an upward reaction RB.k to develop with time at support B. As a consequence, the positive span moments increase with time and the negative moment at support A decreases, as shown in Fig. 8.5b(ii).

306 Members and structures −ve ksh

+ve ksh

Straight

Straight

As A (i)

As B

As

ΔRB.k

L

A (ii)

B

As L

DRB.k

(a) Unrestrained shrinkage deformation and shrinkage–induced reaction at support B Applied load

A

Applied load

B

A

B

RB.0

RB.0 RB.0 + DRB.k

RB.0 + DRB.k First loading, t0 Time tk after shrinkage

(i)

First loading, t0 Time tk after shrinkage

(ii) (b) Redistribution of bending moments caused by shrinkage

Figure 8.5 Effects of shrinkage in a one-fold indeterminate beam.

Of course, the shrinkage-induced actions occur gradually and are therefore relieved by creep. If shrinkage were not accompanied by creep, the time-dependent redistribution of internal actions would be signiﬁcantly greater than it actually is. 8.3.2 Determination of redundants A detailed discussion of the various techniques commonly employed for the analysis of statically indeterminate structures is not attempted here. There are numerous excellent texts on structural analysis, including Refs 2 and 3. In this section, a brief revision of the force method of structural analysis is made and the way in which the method can be used for the time-analysis of indeterminate structures is described and illustrated by example. In the following, the structure is initially assumed to be homogeneous. In the force method, a n-fold indeterminate structure is converted into a statically determinate primary structure by the selection of n internal actions (or external reactions) as redundants and making the corresponding releases. Let the vector of redundant forces be RR . The vector of external loads P applied to the primary structure produces reactions RP at the supports and the external loads (or the load-independent environmental effects such as temperature change or shrinkage) cause displacements of the primary structure at each release uP . These displacements are incompatible with the support

Members and structures

307

conditions of the indeterminate structure and must be eliminated by the unknown redundant forces. If the primary structure is subjected to a unit virtual force at the position of the ˜ Ri = 1, the resulting displacements at each of the n releases are i-th redundant, i.e. R called ﬂexibility coefﬁcients and are denoted fi1 , fi2 , … fin . If ﬂexibility coefﬁcients are determined for unit values of each redundant, an n × n ﬂexibility matrix F may be established, where the term fij is the displacement of the primary structure at release j due to a unit value of the ith redundant. The reactions at the supports of the primary structure caused by unit values of the redundants are also calculated and may be assembled into an m by n matrix RPR where m is the number of reactions in the primary structure. The redundant forces are obtained by solving the following set of simultaneous equations which is generated when compatibility is enforced at each release: F RR = −uP

(8.4)

where, if necessary, support movements could also be included on the right hand side of the equation. The reactions of the statically indeterminate structure are obtained by adding the reactions caused by the redundants (RPR RR ) to the reactions calculated earlier for the released structure RP . That is: R = RP + RPR RR

(8.5)

For a structure with uniform creep characteristics throughout that is subjected to constant sustained loads, the deformation at time τk will be (1 + ϕ) times the deformation at ﬁrst loading τ0 , where ϕ (= ϕ(τk , τ0 )) is the creep coefﬁcient at time, τk , due to a stress ﬁrst applied at τ0 . If the presence of the reinforcement is ignored and if cracking is also ignored, the displacements u at time τk are (1 + ϕ) times their value at τ0 and each term of the ﬂexibility matrix F is also increased by the factor (1 + ϕ). In addition, the reactions R of the statically indeterminate structure do not change and therefore there is no change in the internal actions with time. As has been previously pointed out, this not the case, however, in most concrete structures where the reinforcement layout varies throughout the structure and the extent of cracking also varies. The propped cantilevers shown in Fig. 8.5a are a typical case. The reinforcement is not uniform throughout and, in all probability, parts of the beams are cracked and parts are not. The creep characteristics are therefore far from uniform. In such structures, some creep-induced change in the reactions (and in the internal actions) with time can be expected. In Section 8.3.1, the change in reactions of the members shown in Fig. 8.5a caused by shrinkage warping was also discussed. To calculate the time-dependent change in reactions and internal actions during any time interval (τk – τ0 ), it is ﬁrst necessary to calculate the change in the displacements of the primary structure at each release, uP . The displacements caused by both creep and shrinkage are included here, plus any other displacement that may occur during the time interval, perhaps due to support settlement, additional external loads, losses of prestress, and so on. The AEMM may be used to include time-dependent deformations and an ageadjusted ﬂexibility matrix F can also be determined. Changes in the redundants with time are developed gradually between τ0 and τk and the creep plus elastic displacements

308 Members and structures caused by these gradually applied redundants forces may be calculated using the age-adjusted modulus for concrete Ee (deﬁned in Eq. 4.35) instead of Ec . The ageadjusted ﬂexibility matrix F is therefore formed in exactly the same way as F, except that the displacement (elastic + creep) at each release due to the gradually applied unit force at the position of the ith redundant is calculated using Ee . The time-dependent change in the redundants is obtained by solving the compatibility equations: FRR = −uP

(8.6)

and the change in the reactions of the statically indeterminate structure are: R = RP + RPR RR

(8.7)

where RP is the change in reactions of the primary structure due to any changes of the external loads during the time interval under consideration. For the analysis of a statically indeterminate reinforced or prestressed concrete beam or frame, the procedures outlined in Chapters 4–7 may be used to calculate the deformation (strain and curvature, εr.k and κk ) on any cross-section of the determinate primary frame at any time. When deformations have been determined at several sections, the time-dependent changes in displacement u may be calculated by numerical integration or by virtual work. In this way, the effect of the reinforcement and the inﬂuence of cracking, as well as the effects of creep and shrinkage, can be included directly in the time analysis of an indeterminate member.

Example 8.3 The ﬁnal shrinkage-induced internal actions at time τk in the unloaded and uncracked propped cantilever shown in Fig 8.6 are to be determined. The structure is, of course, one-fold indeterminate, that is, n = 1. Ec = 25,000 MPa; ϕ = 2.5; χ = 0.65; ∗ = −600 × 10−6 ; and E = Ec = 9,524 MPa. εsh e 1+χϕ 300

300

As

A

50

As = 1860 mm2 3000 Region 1

7000 Region 2 Elevation

B

As = 1860 mm2 Region 2

550

500

50

50 Region 1

Sections

Figure 8.6 Dimensions and properties of the beam in Example 8.3 (all dimensions in mm).

Using the procedures outlined in Section 5.4, the age-adjusted effective modulus is used to determine the ﬁnal shrinkage-induced curvature on an

Members and structures

309

otherwise unloaded and unrestrained cross-section in Region 2: (κsh )2 = 0.663 × 10−6 mm−1 . The shrinkage-induced curvature in Region 1 is zero, because each cross-section is symmetrically reinforced (and uncracked). The vertical reaction at support B is selected as the redundant, i.e. RR = VB . The primary structure is therefore a cantilever ﬁxed at support A. The change in the vertical displacement of the primary structure at support B (uB ), due to the shrinkage-induced curvature distribution shown in Fig. 8.7a, is calculated using the second moment area method as: uB =

0.663 × 10−6 × 70002 = 16.24 mm 2 0.663 × 10−6 mm−1 DuB B

A 3000 Region 1

A

B

7000 Region 2

(a) Shrinkage curvature

(b) Deflected shape

Figure 8.7 Shrinkage-induced curvature and deﬂected shape of primary structure in Example 8.3.

The vertical displacement at B due to a gradually applied unit force at B is f11 and is obtained from the curvature diagram shown in Fig. 8.8c, calculated by analysing the uncracked section in the various regions of the cantilever: f11 = 0.1301 × 10−6 ×

10,0002 70002 + (0.1299 − 0.0911) × 10−6 × 3 3

= 4.97 mm/kN B A

10 m

1 kN

(a) Unit load at B

+10

(b) Moment, M (kNm) +0.0911 +0.1301

+0.1299

(c) Curvature (10−6mm−1) f11 (d) Deflected shape

Figure 8.8 Virtual moment and curvature diagram in Example 8.3.

310 Members and structures The redundant VB is calculated from Eq. 8.6 as: f¯11 VB = −uB

from which

VB =

−16.24 = −3.27 kN (i.e. ↓) 4.97

The shrinkage-induced internal actions and external reactions are shown in Fig. 8.9. −32.7 kNm

32.7 kNm A

B

3.27 kN

−3.27 kN

3.27 kN (a) Reactions

(b) BMD

(c) SFD

Figure 8.9 Shrinkage-induced reactions, bending moment and shear force diagrams for Example 8.3.

Example 8.4 The reactions of the one-fold indeterminate propped cantilever of Fig. 8.6 are to be determined at times τ0 and τk . A uniformly distributed load ws = 8 kN/m ﬁrst applied at τ0 is assumed to remain constant with time. The material properties are as for Example 8.3 and the ﬂexural tensile strength of concrete is taken to = 3.0 MPa. be fct.f

1. Calculation of the reactions at time τ0 immediately after the application of w s (a) Ignoring the effects of cracking As in the previous example, the vertical reaction at support B is selected as the redundant, i.e. RR = VB . The 8 kN/m uniformly distributed load produces the following reactions at support A of the primary beam: MA = −400 kNm and VA = 80 kN, therefore:

RP =

−400 MA = 80 VA

If the ﬂexural rigidity EI (= M/κ) is constant throughout the entire span, the vertical displacement at the end of the cantilever at B due to a uniform load ws is: uB = −

ws L4 8EI

Members and structures

311

and the vertical displacement at B due to a unit vertical (upward) force at B (f11 ) and the corresponding reactions of the primary structure are: f11 =

L3 3EI

and

RPR =

MA = L VA = −1

From Eq. 8.4: VB ×

L3 wL4 = 3EI 8EI

and therefore VB =

3wL = 30 kN(↑) 8

The other reactions of the statically indeterminate frame are obtained from Eq. 8.5: ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ MA −400 10 −100 kN.m ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ R = ⎣ VA ⎦ = ⎣ +80 ⎦ + ⎣ −1 ⎦ × 30 = ⎣ +50 kN ⎦ 0 1 +30 kN VB If the effects of cracking are ignored, the bending moment diagram of the indeterminate member immediately after ﬁrst loading is shown in Fig. 8.10. MA = −100.0 5m 3.75 m

− C

A

B +

50.0

56.25

Figure 8.10 Initial bending moment diagram (ignoring cracking) in kNm for Example 8.4.

If the effects of cracking are also ignored in the calculation of deﬂection (which, of course may grossly underestimate the actual deﬂection), the initial curvature on the doubly-reinforced section at support A and on the singly-reinforced section at the mid-span C are calculated using the analysis outlined in Section 5.3 as κA,0 = −0.569 × 10−6 mm−1 and κC,0 = +0.325 × 10−6 mm−1 , respectively. The short-term deﬂection at mid-span vC may be determined using Eq. 8.1b: vC =

10,0002 [−0.569 + 10 × 0.325 + 0] × 10−6 = 2.79 mm 96

312 Members and structures (b) Including the effects of cracking From a short-term cross-sectional analysis of the singly reinforced section in the positive moment region (Region 2), the cracking moment is 65.3 kNm. This is greater than the maximum positive moment in Fig. 8.10 and, therefore, the midspan region is not cracked initially. For the doubly reinforced section at support A (in Region 1), the cracking moment is 70.3 kNm. Therefore, the beam is cracked in the negative moment region near support A. The previous analysis must now be modiﬁed to include the effects of cracking at A. Tension stiffening is not considered here, but could be easily taken into account using the averaging procedure discussed in Section 8.2.3. If the bending moment diagram in Fig. 8.10 is taken as an initial approximation, the extent of cracking is small, with the cracked region extending just 0.625 m from support A. The curvatures at sections in the various regions of the beam are calculated from short-term cross-sectional analyses (Section 5.3 for the uncracked cross-sections and Section 7.2 for the cracked cross-sections) and the instantaneous ﬂexural rigidities (EI = M/κ) are: In Region 1: In Region 2:

Uncracked

(EI)cr.1 = 70.67 × 1012 Nmm2 (EI)uncr.1 = 175.7 × 1012 Nmm2

Uncracked

(EI)uncr.2 = 154.0 × 1012 Nmm2

Cracked

As previously calculated:

−400 MA RP = = +80 VA and the vertical displacement at the end of the primary beam (at B) due to ws = 8 kN/m is found, by moment-area methods or by virtual work, from the curvature diagram shown in Fig. 8.11a and equals uB = −78.5 mm. The displacement at B of the cracked member due to a unit vertical force at B is found from the curvature diagram in Fig. 8.11b and equals f11 = 2.51 mm/kN. From Eq. 8.4: VB =

−uB 78.5 = = 31.3 kN(↑) f11 2.51

and the reactions of the statically indeterminate beam are obtained from Eq. 8.5: ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ −400 10 −87 kN.m MA ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ {R} = ⎣ VA ⎦ = ⎣ 80 ⎦ + ⎣ −1 ⎦ × 31.3 = ⎣ 48.7 kN ⎦ 0 1 31.3 kN VB The bending moment and curvature diagrams after cracking are illustrated in Fig. 8.12. The short-term deﬂection at mid-span may be obtained by virtual work from the curvature diagram in Fig. 8.12 and is vc = 3.17 mm. For this beam, cracking at, and near, the support at A causes a reduction in the negative moment at A, an increase in the positive span moments and a 14 per cent increase in mid-span deﬂection. After initial cracking, moment is shed to the stiffer uncracked parts of the structure. If the load w was increased,

Members and structures

313

w = 8 kN/m A

B

B

A

10 m −400

1 kN

−351.6 −196

A

B 0.625 m 3m 7m Moment (kNm)

−5.66 ×

10−6

+10 Moment (kNm)

−4.975 × 10−6 −2.001 × 10−6 −1.273 × 10−6

+0.0398 × 10−6

−1.116 × 10−6 A

+0.0534 × 10−6

B Curvature (M/EI) (mm−1)

0.1415 ×

(a) Moment and curvature caused by w

10−6

+0.0455 × 10−6

+0.1327 × 10−6 Curvature (M/EI) (mm−1) (b) Moment and curvature caused by a unit load at B

Figure 8.11 Moment and curvature diagrams for cracked primary beam of Example 8.4. 0.625 m

7.0 m

2.375 m

−1.238 × 10−6

MA = −87.5

−58.5 −

5m 3.908 m C

A 22.8

B +

56.3

61.1

(a) Bending moment diagram (kNm)

−0.828 × 10−6

− −0.333 × 10−6 C A 0.130 × 10−6 0.148 × 10−6 0.366 × 10−6

B +

0.397 × 10−6

(b) Curvature diagram (mm−1)

Figure 8.12 Moment and curvature diagrams after cracking in Example 8.4.

cracking would also occur in the positive moment region. With the member more uniformly cracked and the stiffness more uniform in the peak moment regions, the bending moments would redistribute back towards the distribution shown in Fig. 8.10, but the deﬂection would increase signiﬁcantly due to the reduction in the ﬂexural rigidity for Region 2 from (EI)uncr.2 to (EI)cr.2 .

2. Calculation of the reactions at time τk after creep and shrinkage Let the change in reaction at support B be the unknown redundant at time τk , i.e. RR = VB.k . The primary structure (cantilevered beam) is shown in Fig. 8.13a, together with the external loads and the known reactions immediately after ﬁrst

314 Members and structures loading (at τ0 ). Using the procedures outlined in Sections 5.4 and 7.3 for the time analysis of the uncracked and fully-cracked cross-sections, respectively, the curvature diagram at τk after creep and shrinkage is calculated and illustrated in Fig. 8.13b and the curvature diagram due to creep (with shrinkage set to zero) is shown in Fig. 8.13c. The creep and shrinkage characteristics of the concrete are those of Example 8.3 and given in Fig. 8.6. Although not strictly correct, the extent of cracking is assumed to remain unchanged with time. Of course, at ﬁrst loading, the deﬂection of the primary beam at B is zero. But as the primary beam creeps and shrinks under the constant sustained loads shown in Fig. 8.13a, the deﬂection at B becomes non-zero. By numerical integration of the curvature diagrams at time τk (in Fig. 8.13b and c), the deﬂection of the primary cantilever at B is uB = 20.5 mm (upwards) when both creep and shrinkage are considered and uB = 8.49 mm for creep only. −2.153 × 10−6 MA = −87.4 kNm

−0.761 × 10−6

8 kN/m 10 m VB = 31.3 kN

VA = 48.7 kN

3.908 m

0.297 × 10−6 1.086 × 10−6

+0.663 × 10−6

1.796 × 10−6 (b) Curvature of primary beam (mm−1) – creep and shrinkage

(a) Loads on primary beam −1.548 × 10−6

−1.640 × 10−6

−1.029 × 10−6 −0.761 × 10−6

0.297 × 10−6 0.429 × 10−6

3.908 m

1.136 × 10−6

(c) Curvature of primary beam (mm−1) – creep only

Figure 8.13 Load and curvature diagrams of released structure in Example 8.4.

The vertical displacement at the end of the cantilever (at B) at time τk due to a gradually applied unit force at B is f11 and may be calculated by ﬁrst analysing the various cross-sections to determine the long-term curvature. The ﬁnal curvature diagram associated with a unit virtual force at B is shown in Fig. 8.14. A

B

0.625 m

f11

0.1220 × 10−6

+1 +10.0

Loads

2.375 m

0.1771 × 10

Moments

−6

7.0 m

0.0911 × 10−6

0.1299 × 10−6 0.1660 × 10−6

Curvature (mm−1)

Figure 8.14 Moment and curvature at time τk due to gradually applied unit virtual load at B in Example 8.4.

Members and structures

315

The deﬂection at B due to a unit virtual force at B (f11 ) is readily obtained from the curvature diagram using moment-area methods or numerical integration: f11 = 0.1299 ×

7.02 + 0.0911 × 2.375 × 8.188 + (0.1220 − 0.0911) 3

2.375 × 8.583 + 0.1660 × 0.625 × 9.688 + (0.1771 − 0.1660) 2 0.625 × × 9.792 = 5.25 mm/kN 2

×

From Eq. 8.6, the change in the reaction at B with time is: VB = −

uB 20.5 =− = −3.90 kN(i.e. ↓)− for both creep and shrinkage ¯f11 5.25

VB = −

8.49 = −1.62 kN(i.e. ↓)− for creep only 5.25

In Fig. 8.15, the reactions at time τk and the corresponding internal actions are compared with the values immediately after ﬁrst loading. Note that although the MA = −87.4 kNm

MA = −126.0 kNm

8 kN/m 10 m

8 kN/m 10 m

VB = 31.3 kN

VA = 48.7 kN

VA = 52.6 kN Final reactions (at tk)

Initial reactions (at t0)

VB = 27.4 kN

−126.0 kNm

−87.4 kNm

+ 46.9 kNm

+ 61.1 kNm Initial bending moments (at t0)

Final bending moments (at tk)

(a) Initial actions (at t0)

(b) Final actions (at tk) – creep + shrinkage

MA = −103.5 kNm

8 kN/m 10 m VB = 29.7 kN

VA = 50.3 kN Final reactions (at tk) −103.5 kNm

+ 54.9 kNm Final bending moments (at tk) (b) Final actions (at tk) – creep only

Figure 8.15 Initial and ﬁnal reactions and moments in Example 8.4.

316 Members and structures initial cracking at A caused a reduction in the peak negative moment at the ﬁxed support, the effect of creep and shrinkage is to substantially increase the moment at support A and reduce the positive moment at mid-span. In this example, creep causes the magnitude of the moment at A to increase by about 18 per cent (from 87.4 to 103.5 kNm) and shrinkage causes a further increase of 26 per cent (from 103.5 to 126.0 kNm). In the positive moment region, shrinkage-induced tension in the concrete may cause time-dependent cracking and this will reduce the stiffness of the positive moment region resulting in a further increase in the negative support moment and a decrease in the positive span moments. The increase in negative moments will increase the extent of cracking near the support and this, in turn, will cause a slight redistribution of moments from the negative to the positive moment region.

8.3.3 Effects of deformation or settlement at the supports If a statically indeterminate member is subjected to a sudden movement of the supports, changes in the magnitudes of the reactions and internal actions occur. If the imposed deformation at the supports is kept constant, the reactions and internal actions gradually change with time due to relaxation. If the support deformations occur gradually, the changes in reactions and internal actions also occur gradually. The simultaneous development of creep causes a relaxation of the internal forces as the support movements are taking place. Therefore, the reactions induced in an indeterminate member by a gradual deformation at one or more supports tend to increase from zero (at the commencement of movement) to a maximum value as the maximum deformation is approached, and then reduce as creep continues after the support deformation has ceased. Consider the propped cantilever beam AB subjected to a sudden support settlement δB (τ0 ) at time τ0 , as shown in Fig. 8.16. The time-dependent reactions introduced at the supports are also shown. Immediately after the support settlement at time τ0 , the vertical reaction at B can be determined using the force method. For a beam with uniform cross-section throughout: RB (τ0 ) =

3Ec I δB (τ0 ) L3

(8.8)

where I is the second moment of area of the transformed section about its centroidal axis. The change in the reaction at support B that occurs with time over the time period τk − τ0 is: RB = RB (τk ) − RB (τ0 ) MA(t)

(8.9)

A

B dB(t0)

RA(t) L

RB(t)

Figure 8.16 Time-dependent reactions caused by a support settlement.

Members and structures

317

and may be determined using the procedure outlined in Section 8.3.2 (and Eqs 8.6 and 8.7). If the support settlement δB (t) is gradually applied, the reaction RB (t) increases gradually with time. If the settlement occurs at the same rate as the creep of the concrete, the reaction at B in a member of uniform cross-section may be approximated by: RB (t) =

3Ee I¯ δB (t) L3

(8.10)

where I is the second moment of area of the age-adjusted transformed cross-section about its centroidal axis. After the support settlement reaches its maximum value at some time τ1 , the subsequent change in the reaction with time (at t > τ1 ), RB = RB (t) − RB (τ1 ), may be calculated using Eq. 8.6.

Example 8.5 The initial and ﬁnal internal actions in the unloaded and uncracked member shown in Fig. 8.17 are to be determined, if the support at B suffers a vertical displacement of 20 mm, as shown. 300

MA(t)

A

B 20 mm

50

As = 1860 mm2

500 RA(t)

RB(t)

As = 1860 mm2

50

10 m Elevation

Cross-section

Figure 8.17 Details of beam subjected to support settlement in Example 8.5.

(a) If the support settlement occurs suddenly at 28 days Maternal and cross-sectional properties are Ec (τ0 ) = 25,000 MPa; I = 7028 × 106 mm4 ; ϕ(∞, τ0 ) = 2.8; χ (∞, τ0 ) = 0.65. The reaction at B at age τ0 , immediately after the support displacement, is found using Eq. 8.8: RB (τ0 ) =

3 × 25,000 × 7028 × 106 × 20 = 10.54 kN ↓ 10,0003

and the internal bending moment varies from zero at B to −105.4 kNm at A. The initial curvature varies from zero at B to κA.0 = MA /Ec I = −0.60 × 10−6 mm−1 at A as shown in Fig. 8.18b. It is assumed here that the member remains uncracked throughout. The ﬁnal curvature at end A, caused by the sustained

318 Members and structures moment of −105.4 kNm, is calculated using the cross-sectional analysis of Section 5.4 and equals κA.k = −1.434 × 10−6 mm−1 , as shown in Fig 8.18b. The creep-induced change of curvature at end A is therefore κA.k − κA.0 = −0.834 × 10−6 mm−1 . If the displaced beam is released at B, the creep induced curvature causes a gradual displacement at end B given by: 0.834 × 10−6 × 10,0002 = 27.8 mm ↓ 3

uB =

For this member, the age-adjusted effective modulus is Ee = 8865 MPa and the second moment of area of the age-adjusted transformed cross-section about its centroidal axis is I = 10,410 × 106 mm4 . The vertical displacement caused by a gradually applied unit load (1 kN) at B is: f11 =

L3 3Ee I

=

10,0003 = 3.61 × 10−3 mm/N 3 × 8865 × 10,410 × 106

and the change in the reaction at B with time is: RB =

uB f 11

=

27.8 = 7701 N = 7.70 kN ↑ 3.61 × 10−3

The ﬁnal reaction at B is therefore: RB (τk ) = RB (τ0 ) + RB = 10.54 − 7.70 = 2.84 kN(↓) and the moment at A relaxes from −105.4 kNm at τ0 to a ﬁnal value of −28.4 kNm.

MA(t) = 105.4 kNm A

B

−0.834 20 mm

Creep induced initial

−0.600

RB(t0) =10.54 kN

RB(t0) = 10.54 kN 10 m

(b) Initial and final curvature of released structure (×10−6 mm−1)

(a) Initial reactions due to 20 mm support settlement 20 mm DuB

(c) Final deformation of released structure

Figure 8.18 Actions and deformations of released primary beam in Example 8.5.

Members and structures

319

(b) If support settlement of 20 mm occurs gradually between τ0 = 28 days and τ1 = 180 days It is here assumed that the rate of settlement is similar to the rate of creep and the following material properties are assumed: For concrete loaded at 28 days: Ec (28) = 25,000 MPa; ϕ(180, 28) = 1.5; ϕ(∞, 28) = 2.8; χ(180, 28) = χ (∞, 28) = 0.65 For concrete loaded at 180 days: Ec (180) = 30,000 MPa; ϕ(∞, 180) = 1.0; χ (∞, 180) = 0.65. The age-adjusted effective modulus at age 180 days due to a stress ﬁrst applied at 28 days is Ee = 12,660 MPa and the second moment of area of the corresponding age-adjusted transformed cross-section is I = 8841 × 106 mm4 . The reaction at B at τ1 = 180 days, when δB reaches 20 mm, is calculated using Eq. 8.10: RB (180) =

3 × 12,660 × 8841 × 106 × 20 = 6720 N = 6.72 kN(↓) 10,0003

and the corresponding moment at the ﬁxed support A is −67.2 kNm. If the displacement at B remains constant at 20 mm after τ1 = 180 days, the reactions and internal actions will gradually decrease, in the same manner as in case (a). The change in reaction at B that occurs after τ1 , RB , is selected as the redundant. The creep-induced curvature κA that develops at A in the primary beam due to a sustained moment of −67.2 kNm (after t = 180 days) is calculated using the cross-sectional analysis presented in Section 5.4. With ϕ(∞, 180) = 1.0 and χ (∞, 180) = 0.65, κA is equal to −0.223 × 10−6 mm−1 . The resulting timedependent change in deﬂection of the primary beam at B is: uB =

−0.223 × 10−6 × 10,0002 = −7.43 mm (i.e. ↓) 3

The appropriate properties of the age-adjusted transformed section are Ee = 18,180 MPa and I = 7725 × 106 mm4 . Due to a gradually applied unit load at B: f11 =

10,0003 = 2.37 × 10−3 mm/N 3 × 18,180 × 7725 × 106

The change in the reaction at B, which occurs after τ1 = 180 days, is therefore: RB = −

−7.43 = 3140 N = 3.14 kN(↑) 2.37 × 10−3

and the ﬁnal reaction at B is therefore RB (∞) = 6.72 − 3.14 = 3.58 kN (↓). The corresponding bending moment at the ﬁxed end of the member MA (∞) = −35.8 kNm.

320 Members and structures

Bending moment at support A MA (kNm)

Plots of MA versus time for both the sudden support settlement and the gradual support settlement are shown in Fig. 8.19.

100 (a) Sudden support settlement 80 60 40 (b) Gradual support settlement

20

Time, t 0 28

180

Figure 8.19 Time variation of moment due to sudden and gradual support settlement in Example 8.5.

8.3.4 Further effects of creep in prestressed construction Although creep in continuous members causes a dramatic reduction of the internal actions caused by imposed deformation (as shown in curve (a) of Fig. 8.19), the effects of creep on the redistribution of internal actions in continuous members subjected to imposed loads is less pronounced, but still signiﬁcant (as demonstrated in Example 8.4). In general, internal actions are redistributed from the regions with a higher creep rate to the regions with the lower creep rate. In Example 8.4, with the rate of change of curvature due to creep in the singly-reinforced mid-span Region 2 greater than the rate of change of curvature in the doubly-reinforced Region 1, creep causes a decrease in the positive span moments with time and an increase in the negative moments at the continuous support (see Fig. 8.15). The internal actions caused by prestress are also affected by creep of concrete. They are obviously affected by the losses of prestress caused by creep and these losses can vary from near zero, when the member is cracked at the level of the tendon, to as much as 20 per cent or more, when the member is heavily prestressed at an early age and the concrete compressive stress at the level of the bonded tendon is high. The hyperstatic reactions induced by prestress in indeterminate structures are in fact imposed loads applied to the structure at the supports and the resulting secondary moments are affected by creep. If the structural system changes after the application of some of the prestress, creep may cause a change in the hyperstatic reactions. As an example, consider the two-span beam shown in Fig. 8.20. The beam is fabricated by erecting two simply-supported prismatic precast concrete girders (of constant cross-section) over the two spans of length L. Each girder contains a single layer of straight pretensioned strands at a

Members and structures

321

In-situ joint e

A

B Pretensioning tendon L

C Precast, pretensioned girder L

Figure 8.20 Providing continuity at a continuous support.

constant eccentricity e below the centroidal axis of the cross-section. The structure is then rendered continuous by casting an in-situ joint over the interior support. Any time-dependent defomations in the members will be restrained by the imposed ﬁxity at the interior support and hyperstatic reactions will develop with time, together with the associated secondary moments and shears. Before the in-situ joint in Fig. 8.20 is cast, the two-precast girders are simply supported, with zero deﬂection but some non-zero slope at the interior support at B. Immediately after the joint is fabricated and continuity is established, the internal primary moment imposed by the prestress on each cross-section is Pe about the centroidal axis, but the initial secondary moment at B (and elsewhere) is zero. With time, creep will cause a gradual change in the curvature on each cross-section. If the support at B was released so that a vertical displacement at B was possible, the member ABC would gradually deﬂect upwards at B due to the creep-induced hogging curvature associated with the primary moment Pe on each cross-section. If it is assumed that the creep characteristics are uniform and the prestressing force is constant throughout, the time-dependent curvature caused by creep on each crosssection can be determined using the procedure presented in Section 5.4. For lightly reinforced cross-sections, the creep-induced curvature (κk )cr may be taken as a product of the instantaneous curvature and the creep coefﬁcient (Eq. 8.11a) and the upward displacement at B is given by Eq. 8.11b: (κk )cr = uB (τk ) =

Pe ϕ(τk , τ0 ) Ec I

(8.11a)

(κk )cr L2 2

(8.11b)

where I is the second moment of area of the transformed section about its centroidal axis. In Eq. 8.11a, it is assumed that the restraint offered to creep by the bonded reinforcement is insigniﬁcant. If the amount of bonded reinforcement is signiﬁcant, a more accurate approximation may be made by dividing the creep coefﬁcient in Eqs 8.11 by the parameter α deﬁned in Section 3.6.6 and, for uncracked cross-sections, speciﬁed in Eq. 3.32b.

322 Members and structures The deﬂection at B caused by a unit value of the vertical redundant reaction force gradually applied at the release at B may be calculated using the procedures of Section 8.3.2. An approximation for the time-dependent ﬂexibility coefﬁcient associated with the release at B is given by: L3 [1 + χ (τk , τ0 )ϕ(τk , τ0 )] L3 = f¯11 = 6Ec I 6 Ee I

(8.12)

The redundant force at B that gradually develops with time RB (τk ) is obtained from Eq. 8.6: RB (τk ) = −

uB (τk ) 3Pe ϕ(τk , τ0 ) ≈− ¯f11 L 1 + χ(τk , τ0 )ϕ(τk , τ0 )

= RB

ϕ(τk , τ0 ) 1 + χ(τk , τ0 )ϕ(τk , τ0 )

(8.13)

where RB is the hyperstatic reaction that would have developed at B if the structure was initially continuous and later prestressed with a straight tendon of constant eccentricity e. In general, if R is any hyperstatic reaction or the restrained internal action that would occur at a point due to prestress in a continuous member and R(t) is the corresponding creep-induced value if the member is made continuous after the application of prestress, then: RB (t) ≈

ϕ(τk , τ0 ) R 1 + χ(τk , τ0 )ϕ(τk , τ0 )

(8.14)

If the creep characteristics of the concrete are uniform throughout the structure, then Eq. 8.14 may be applied to systems with any number of redundants. Providing continuity at the interior supports of a series of simple precast beams, not only restrains the time-dependent deformation caused by prestress, but also restrains the deformation caused by external loads. For all the external loads applied after the continuity is established, the effects can be calculated by moment distribution or an equivalent method of structural analysis. Under the loads applied to the simplysupported beams prior to casting the joints (such as the self-weight of the precast beams), the moments at each interior support are initially zero. However, after the joint has been cast, the creep-induced deformations resulting from these selfweight moments are restrained and moments develop with time at the supports. For the two-span beam shown in Fig. 8.20, the initial moment at the support B due to self-weight is zero. However, if the beam had initially been continuous over the interior support, the moment at B would have been MB = wsw L2 /8. The moment that develops with time due to creep at support B due to creep and self-weight is: MB (t) ≈

ϕ(τk , τ0 ) MB 1 + χ(τk , τ0 )ϕ(τk , τ0 )

Members and structures

323

Example 8.6 Consider two simply-supported pretensioned concrete planks, erected over two adjacent spans as shown in Fig. 8.20. An in-situ reinforced concrete joint is cast at the interior support, to provide continuity. Each plank is 1000 mm wide by 150 mm thick and pretensioned with straight strands at a constant depth of 110 mm below the top ﬁbre, with Ap = 400 mm and Pp,init = 500 kN. A typical cross-section is shown in Fig. 8.21. The span of each plank is L = 6 m. If it is assumed that the continuity is provided immediately after the transfer of prestress, the reactions that develop with time due to creep are to be determined. For convenience, and to better illustrate the effects of creep in this situation, shrinkage is not considered and the self-weight of the planks is also ignored. The material properties are: Ec = 30,000 MPa; fct = 3.0 MPa; ϕ(τk , τ0 ) = 2.0; χ (τk , τ0 ) = 0.65; εsh = 0; and Ee = 13,040 MPa. 1000 150 110

Ap = 400 mm2 Pp,init = 500 kN

Figure 8.21 Cross-section of planks in Example 8.6 (all dimensions in mm).

Immediately after transfer, and before any creep has taken place, the curvature on each cross-section caused by the eccentric prestress may be calculated using the procedure outlined in Section 5.3 giving κ0 = −2.02 × 10−6 mm−1 . The top and bottom ﬁbre concrete stresses are σtop,0 = 1.30 MPa and σtop,0 = −7.81 MPa, so that cracking has not occurred. In the absence of any restraint at the supports, the curvature on each crosssection would change with time due to creep from κ0 to κk = −5.81×10−6 mm−1 (calculated using the procedure outlined in Section 5.4). If the support at B in Fig. 8.20 was removed, the deﬂection at B (uB (τk )) that would occur with time due to the change in curvature caused by creep ((κk )cr = κk −κ 0 = −3.79 × 10−6 mm−1 ) can be calculated from Eq. 8.1b for the 12 m long planks and is also given by Eq. 8.11b: uB (τk ) =

−3.79 × 10−6 × 60002 = −68.2 mm (i.e. upward) 2

The deﬂection at B caused by a unit value of the vertical redundant reaction force gradually applied at the release at B is calculated using the procedures of Section 8.3.2 and for this example is given by Eq. 8.12. With the second moment of area of the age-adjusted transformed cross-section I = 288.3 × 106 mm4 , Eq. 8.12 gives: L3 60003 f¯11 = = = 9.58 × 10−3 6 Ee I¯ 6 × 13,040 × 288.3 × 106

324 Members and structures and the redundant force at B that gradually develops with time, RB (τk ) is therefore: RB (τk ) = −

uB (τk ) −68.2 =− = 7124 N ¯f11 0.00958

The reaction that would have developed at B due to prestress immediately after transfer if the member had initially been continuous is RB = 8621 kN and the approximation of Eq. 8.14 gives: RB (τB ) ≈

2.0 × 8621 = 7497 N 1 + 0.65 × 2.0

In this example, Eq. 8.14 gives a value for RB (τk ) that is within 6 per cent of the value determined above and provides a quick and reasonable estimate of the effects of creep. The secondary moment at B that develops with time due to prestress is 21.4 kNm and this is 83 per cent of the secondary moment that would have developed if the two planks had been continuous at transfer.

8.4 Two-way slab systems 8.4.1 Discussion The design of suspended concrete slab systems is complicated by the difﬁculties involved in estimating the service load behaviour. It is relatively easy to ﬁnd a load path and reinforce a slab to satisfy the requirements of adequate strength. Slabs are usually very ductile, highly indeterminate members that are capable of considerable moment redistribution as the ultimate load is approached. The distribution of moments in a statically indeterminate slab at failure is very much dependent on the reinforcement pattern and, therefore, on the load path assumed in design. However, in the design for serviceability, the distribution of moments and the prediction of deﬂection at service loads are far more uncertain. The distribution of moments varies with time and depends on the extent of cracking, the post-cracking stiffness of the various parts of the slab, the level of creep and shrinkage and the restraint provided at the supports. As outlined in the preceding pages, the initial and time-dependent deformations and the extent of cracking in concrete structures depend primarily on the non-linear and inelastic properties of concrete and, as such, are difﬁcult to predict with conﬁdence. The problem is exacerbated in the case of slabs which are typically thin in relation to their spans and are therefore more deﬂection sensitive. It is stiffness rather than strength that controls the design of most reinforced and prestressed concrete slab systems. The ﬁrst step in the design of a two-way slab panel is the initial selection of the slab thickness. A reasonable ﬁrst estimate is desirable since, in many cases, the slab selfweight is a large portion of the total service load. The initial estimate is often based on personal experience or on recommended maximum span-to-depth ratios or minimum thickness requirements, such as those presented in Section 3.5. While providing a useful starting point in design, such a selection does not necessarily ensure serviceability. Deﬂections at all critical stages in the history of the slab must be calculated and

Members and structures

325

the magnitudes limited to acceptable design values. Failure to adequately predict deﬂections has frequently resulted in serviceability problems (Ref. 4). The procedures discussed so far in this chapter have been concerned with the prediction of the in-service behaviour of line members, such as beams, one-way slabs and frames. For the calculation of two-way slab deﬂections, several additional problems need to be overcome. The three-dimensional nature of the slab, the less well deﬁned inﬂuence of cracking and tension stiffening and the development of biaxial creep and shrinkage strains must all be modelled adequately. In addition, the ﬁnal deﬂection of a slab depends very much on the extent of initial cracking which, in turn, depends on the construction procedure (the shoring and reshoring sequence), the amount of early shrinkage, the temperature gradients in the ﬁrst few weeks after casting, the degree of curing and so on. Many of these parameters are, to a large extent, outside the control of the designer. In ﬁeld measurements of the deﬂection of many identical slab panels (Refs 5 and 6), a large variability was reported. Deﬂections of identical panels after one year differed by over 100 per cent in some cases. These differences can be attributed to the different conditions that existed in the ﬁrst few weeks after casting of each slab, including differences in both the applied load and the environmental conditions. In more recent laboratory tests on large-scale ﬂat slabs, a change in deﬂection at least as large as that caused by the full design live load was observed after exposing the top surface of a dry slab to rainwater (Ref. 7). Nevertheless, various approximate methods are available that may be used to predict ball-park estimates of the deﬂection of two-way slabs, making use of the cross-sectional analyses presented in Chapters 4–7. By varying the amount of early cracking, for example by varying the tensile strength of concrete, upper and lower bounds on deﬂection can be obtained. Some approximate procedures for deﬂection calculation are reviewed in the following sections. 8.4.2 Slab deﬂection models In view of the complexities and uncertainties involved in estimating the service load behaviour of two-way slab systems, great accuracy in the calculation of deﬂection is neither possible nor warranted. Nevertheless, numerous approximate techniques are available for the prediction of moments and deformations in concrete slab systems. These range from relatively simple procedures to sophisticated research models. The small deﬂection theory of elastic plates can be used to predict slab deﬂections. Deﬂection coefﬁcients for elastic slabs with ideal boundary conditions and subjected to full panel loading have been presented by Timoshenko and Woinowsky-Krieger (Ref. 8). Many more simple models involve the analysis of orthogonal slab strips. The deﬂection of the slab panel is approximated by the sum of the deﬂection components of one or more slab strips (see Refs 9–15). The ﬁnite-element method is perhaps the most powerful and potentially the most accurate tool for the analysis of concrete slabs. The basic method is well established and has been described in many text books. Since the early 1970s, many investigators have developed non-linear ﬁnite-element models to study the short-term service load behaviour of reinforced concrete slabs. A number of researchers extended their models to handle the time-dependent effects of creep and shrinkage (e.g. Refs 16–18). Today numerous commercial ﬁnite element software packages are available to undertake non-linear analysis of slabs at service loads. The treatment of time effects in these

326 Members and structures computer packages ranges from rational and reliable to crude and unreliable. Users of any commercial program should be aware of the assumptions made in the modelling of material non-linearity, particularly relating to cracking, creep and shrinkage, and make a rational assessment of the reliability of the output. However, ﬁnite element modelling of two-way slab systems, even with the most reliable of software, is time consuming and generally unsuitable for routine use in structural design. However, it is a useful research tool to examine the effects of various parameters on slab behaviour and to generate the parametric data necessary for the development of more simple, design-oriented procedures for the estimation of slab deﬂections. Such parametric studies have been reported elsewhere (Ref. 17) and have led to the development of simple, design-oriented methods for the deﬂection control of slabs (Ref. 15). The ﬁnite-element model described in Ref. 17 has been used for the calibration of slab stiffness factors in the following section. 8.4.3 Two-way edge-supported slabs This section deals with the prediction of the deﬂection of two-way rectangular slab panels that are continuously supported on all four edges by beams or walls and that carry a uniformly distributed load. The slab panel may be either continuous or discontinuous on each edge. A simple and useful estimate of deﬂection may be made using the so-called crossing beam analogy. This involves the consideration of a pair of orthogonal slab strips of unit width spanning through the centre of the panel as shown in Fig. 8.22. Each slab strip carries only part of the transverse load w on the slab. By equating the mid-span deﬂection of each slab strip and assuming that the entire transverse load is carried by bending in the two orthogonal directions, the fraction of load carried in the short-span direction γ ∗ is easily determined. If each strip is initially assumed to be uncracked: γ∗ =

L4y λL4x + L4y

(8.15)

where λ depends on the support conditions of the panel and is given by: λ = 1.0 λ = 1.0 λ = 2.0 λ = 0.5 λ = 2.5 λ = 0.4 λ = 5.0 λ = 0.2

for 4 edges continuous discontinuous for 2 adjacent edges discontinuous for 1 long edge discontinuous for 1 short edge discontinuous for 2 long + 1 short edge discontinuous for 2 short + 1 long edge discontinuous for 2 long edges discontinuous for 2 short edges discontinuous.

The deﬂection of the slab may be estimated conservatively by calculating the initial and time-dependent deﬂection of the shorter span slab strip subjected to a uniformly distributed load, γ ∗ w. However, this ignores the torsional stiffness of the slab and violates compatibility at all but the slab centre. As a consequence, the predicted deﬂection may be signiﬁcantly greater than the actual deﬂection. Using the non-linear

Members and structures

327

Lx = short span Ly = long span

1m

Equivalent slab strip

Panel is continuously supported along all edges

Figure 8.22 Orthogonal slab strips in an edge-supported slab.

ﬁnite-element model described in Ref. 17, a slab stiffness factor has been calibrated which may be used to adjust the stiffness of the shorter span beam, so that the deﬂection of the slab panel is predicted more accurately. In Table 8.4, this slab stiffness factor is combined with the value of γ ∗ (as given by Eq. 8.15). The deﬂection of the panel may be estimated by analysing a unit wide one-way slab strip in the short span direction with the same boundary conditions as the relevant slab edges and carrying uniformly distributed load of γ ∗ w. For each possible boundary condition, γ ∗ depends on the aspect ratio Ly /Lx and may be interpolated from Table 8.4. If the slab edges are supported by beams, the average deﬂection of the supporting beams along the long edges must be calculated and added to the slab strip deﬂection to obtain the total deﬂection at the centre of the panel. Table 8.4 Values of γ ∗ for two-way edge-supported slabs Value of γ ∗ Ly /Lx

4 edges continuous 1 short edge discontinuous 1 long edge discontinuous 2 short edges discontinuous 2 long edges discontinuous 2 adjacent edges discontinuous 2 short + 1 long edge discontinuous 2 long + 1 short edge discontinuous 4 edges discontinuous

1.0

1.25

1.5

2.0

5.0

0.48 0.60 0.31 0.74 0.15 0.45 0.55 0.22 0.36

0.70 0.78 0.50 0.87 0.28 0.66 0.71 0.36 0.50

0.84 0.91 0.69 0.95 0.41 0.79 0.81 0.50 0.60

0.94 0.97 0.87 0.99 0.65 0.93 0.94 0.72 0.80

1.00 1.00 1.00 1.00 0.97 1.00 1.00 1.00 1.00

Example 8.7 The maximum ﬁnal deﬂection at the mid-span of a 6 by 8 m exterior panel of a beam and slab ﬂoor system is to be calculated. The slab panel is 150 mm thick and forms part of the ﬂoor of a retail store. The panel edges are continuously supported by stiff beams. The design moments in the slab have been

328 Members and structures determined from moment coefﬁcients speciﬁed in the local building code and the reinforcement has been calculated to satisfy the design objective of adequate strength. Top and bottom reinforcement plans are shown in Fig. 8.23, together with the relevant material properties. All reinforcement bars are Australian Class N (normal ductility) 12 mm diameter deformed bars spaced at centres shown in millimetres. Bars in the short-span direction are placed closest to the bottom of the slab and closest to the top, as shown, with the effective depth d = 150 − 20 − 6 = 124 mm. 8m

8m

A

D

D

A th

st

N12@300 (4 )

N12@180 (1 )

6m

rd

N12@170 (3 )

nd

N12@230 (2 )

B

th

N12@130 (4 )

C

Stiff beams

N12@170 (3rd)

(a) Bottom reinforcement plan

B

C

(b) Top reinforcement plan

f c′ = 25 MPa ; Ec = 25,000 MPa ; f* = 2.8 ; c* = 0.8 ; e*sh =

−0.0006 ; fy = 500 MPa ; Es = 200,000 MPa ; ft = 2.0 MPa ; Minimum concrete cover = 20 mm

Figure 8.23 Details of 150 mm thick slab panel of Example 8.7.

The slab carries a superimposed dead load of gsup = 1.5 kPa, in addition to its own self-weight gsw , and the speciﬁed live load q is 5.0 kPa. For a retail store, the service load factors are taken as (refer to Section 3.3) ψ1 = 0.6 (for short-term loads) and ψ2 = 0.3 (for long-term loads). If reinforced concrete is taken to weigh 24 kN/m3 , then the sustained load is: wsus = gsw + gsup + ψ2 q = 24 × 0.15 + 1.5 + 0.3 × 5.0 = 6.6 kPa and the variable load is: wvar = (ψ1 − ψ2 )q = (0.6 − 0.3) × 5.0 = 1.5 kPa The slab panel is discontinuous on one long edge only, with an aspect ratio of Ly /Lx = 1.33, and from Table 8.4 γ ∗ = 0.56. A 1 m wide slab strip spanning in the short-span direction through the slab centre is to be analysed. The slab strip is considered to be continuous at one end and simply-supported at the other, as shown in Fig. 8.24a. The analysis of such a member was presented in Example 8.4. Assume the bending moment produced by the maximum short-term load on the strip (i.e. γ ∗ (wsus + wvar ) = 4.54 kN/m) is as shown in Fig. 8.24b.

Members and structures MBC = −20.0 kNm/m

N12@300 = 367 mm2/m

N12@130 = 846 mm2/m

g *w = 4.54 kN/m 150 mm

B-C 6m

N12@180 = 611 mm2/m A-D

329

A-D

B-C Mmid-span = 10.43 kNm/m Mmax = 11.65 kNm/m

(a) Elevation

(b) Bending moment diagram

Figure 8.24 Elevation of slab strip and moment diagram in Example 8.7.

From a short-term cross-sectional analysis using the approach outlined in Section 5.3, the cracking moments for this 150 mm thick slab at mid-span at ﬁrst loading (with zero shrinkage) and at the interior support are +9.89 and −10.09 kNm/m. It is evident that both the positive and negative moment regions of the slab will crack under the full service load. The initial and time-dependent curvatures at each support and at mid-span caused by the sustained load γ ∗ wsus = 3.70 kN/m and the short-term curvatures caused by the variable load γ ∗ wvar = 0.84 kN/m are calculated using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked sections and Sections 7.2 and 7.3 for the cracked sections and are summarised in Table 8.5. From the uncracked analyses, the moments required to produce an extreme ﬁbre tensile stress in the concrete of fct = 2.5 MPa at ﬁrst loading τ0 and at τk are readily determined and given in Table 8.5. Tension stiffening is accounted for using the distribution factor ζ given in Eq. 8.3 and the average curvature κavge at each critical section due to each loading is calculated using Eq. 8.2 and is also given in Table 8.5. Table 8.5 Uncracked, cracked and average curvature at critical sections in Example 8.7. At continuous support

At mid-span

At discontinuous support

At ﬁrst loading, τ0

Final at τk

At ﬁrst loading, τ0

Final at τk

At ﬁrst Final at loading, τ0 τk

Cracking moment, Mcr (kNm/m)

−10.09

−4.64

9.89

5.99

–

–

Max. moment, Ms∗ (kNm/m)

−20.0

−20.0

11.65

11.65

0

0

Distribution factor, 0.746 ζ (Eq. 8.3)

0.946

0.279

0.736

0

0

Due to γ ∗ wvar : κuncr (mm−1 )

−0.50 × 10−6

−0.50 × 10−6

0.27 × 10−6

0.27 × 10−6 0

0

(mm−1 )

−2.18 × 10−6

−2.18 × 10−6

1.48 ×

10−6

1.48 × 10−6 0

0

κavge (mm−1 )

−1.75 × 10−6

−2.09 × 10−6

0.61 × 10−6

1.16 × 10−6 0

0

Due to γ ∗ wsus + shrinkage: κuncr (mm−1 ) κcr (mm−1 )

−2.21 × 10−6 −9.60 × 10−6

−9.20 × 10−6 −20.0 × 10−6

1.17 × 10−6 5.33 × 10−6

6.52 × 10−6 0 14.8 × 10−6 0

0.77 × 10−6 –

κavge (mm−1 )

−7.42 × 10−6

−19.4 × 10−6

2.33 × 10−6

12.6 ×−6

0.77 × 10−6

κcr

0

330 Members and structures The short-term deﬂection at mid-span due to the variable loading at time τk is obtained from Eq. 8.1b: (vc )var =

60002 (−2.09 + 10 × 1.16 + 0) × 10−6 = 3.6 mm 96

and the long-term deﬂection due to the sustained load and shrinkage is (vc )sus =

60002 (−19.4 + 10 × 12.6 − 0.77) × 10−6 = 39.6 mm 96

The maximum total panel deﬂection is therefore (vc )max = (vc )var + (vc )= sus 43.2 mm. With a maximum deﬂection of span/130, this slab is unserviceable for most applications and a thicker slab would almost certainly be required for this ﬂoor system.

8.4.4 Flat slabs In this section, a simple method is presented for predicting the deﬂection at the midpanel of a uniformly loaded two-way column-supported ﬂat slab. The basic procedure is known as the wide beam method (or equivalent frame method) and was formalised by Nilson and Walters (Ref. 19). It is assumed here that the design bending moments in each direction are known and that the quantity and layout of the reinforcement in each region of the slab are also known: that is, the slab has been designed for strength and an estimate of deﬂection is now required. The basis of the method is illustrated in Fig. 8.25. For the deﬂection calculation, the deformation of a slab panel in one direction at a time is considered. The contributions in each direction are then added to obtain the total deﬂection. In Fig. 8.25a, the slab is considered to act as a wide, shallow beam of width equal to the panel dimension Ly and span equal to Lx and carrying the entire load in the x-direction. This wide beam is assumed to rest on unyielding supports. Because of variations in moment and ﬂexural rigidity across the width of the slab, all unit strips in the x-direction will not deform identically. Moments, and hence curvatures, in the regions near the column lines (the column strip) are greater than in the middle strips. The deﬂection on the column line is therefore greater than that at the panel centre. This is particularly so, when, as is usually the case, the column strips are cracked and the middle strips are uncracked. The slab is next considered to act as a wide shallow beam carrying the entire load in the y-direction as shown in Fig 8.25b. Once again, the effect of variation of moment and ﬂexural rigidity across the panel is shown. The mid-panel deﬂection is taken to be the sum of the average mid-span deﬂection of the column strips in one direction (usually taken as the long-span direction) and the mid-span deﬂection of the middle strip in the other direction (Fig. 8.25c). That is:

vcx1 + vcx2 vmax = + vmy (8.16) 2

Members and structures

331

y

Assumed support line

vcx2 vmx

vcx1 Lx

Ly

y Assumed support line

x

(a) x–direction bending

vmy vcy2 Lx

Ly

y x vmax

(b) y–direction bending

Lx

Ly (c) Two-way bending x

Figure 8.25 Deﬂection components of a ﬂat slab (Ref. 19).

The method is fully compatible with the equivalent frame method of moment analysis (Ref. 20). The deﬁnition of column and middle strips, the longitudinal moment distribution, lateral moment distribution coefﬁcients and other details are the same as for the moment analysis, so that in design most of the information required for the estimation of deﬂection has been previously calculated. With the moment diagrams for the column and middle strips known, it is a simple matter to determine the curvatures at the supports and at the mid-span of each strip, using the cross-sectional analyses of Chapters 5 and 7. The initial and time-dependent strip deﬂections can be calculated using Eq. 8.1b. For ﬂat slabs, the span in Eq. 8.1b may be taken to be the centre to centre distance between columns or the clear span (face to face of columns) plus the slab depth, whichever is smaller.

Example 8.8 The maximum total deﬂection at the mid-point of a square interior panel of the ﬂat plate shown in Fig. 8.26 is to be calculated. The slab is 200 mm thick and supports a sustained service load of wsus = 6.3 kPa (which includes self-weight) and a variable live load of wvar = 3.0 kPa. The column and middle strips in each direction are 3575 mm wide. The tensile reinforcement quantities in the x-direction column strip and y-direction middle strip are given in Table 8.6. The steel in the x-direction is placed ﬁrst and

332 Members and structures f c′

Column strip

= 25 MPa; Ec = 25,000 MPa;

fct = 3.0 MPa; fy = 500 MPa; f* =

2.5;

c* =

0.65;

e*sh =

Middle strip

7.15 m 6.75 m

−0.0006

y

D = 200 mm

x

Column strip

Effective span, Le = Ln + D = 6.95 mm

6.75 m 7.15 m

Figure 8.26 Slab details and material properties for Example 8.8.

last (i.e. closest to the top and bottom surfaces of the slab) and the steel in the y-direction is placed in the second and third layers. If 20 mm cover and 16 mm diameter bars are assumed, the effective depths in each direction are: dx = 200 − 20 − 8 = 172 mm dy = dx − 16 = 156 mm Also shown in Table 8.6 are the peak positive and negative in-service bending moments caused by wsus +wvar in each strip. These were calculated in accordance with the direct design method of slab design (see Ref. 20). Table 8.6 Steel quantities and in-service moments for Example 8.8 Column strip (x-direction)

Middle strip (y-direction)

Negative Positive Negative moment region moment region moment region Ast (mm2 ) 5420 Msus+var (kNm) −196

2280 85

1950 −66

Positive moment region 1650 56

Column strip deﬂection (x-direction) At the support The maximum in-service moment in the column strip at the support (due to wsus + wvar ) is −196 kNm and, from the cross-section analysis of Section 5.3, the cracking moment at ﬁrst loading is −80.0 kNm and after all shrinkage is −32.8 kNm. The critical cross-section at the support will obviously be cracked. The ﬁnal time-dependent curvature at the support caused by the moment due to the sustained load (Msus = −132.8 kNm) plus shrinkage and the short-term curvature caused by the moment due to the variable load (Mvar = −63.2 kNm) are calculated using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked section and Sections 7.2 and 7.3 for the cracked section and are

Members and structures

333

summarised below. For the inclusion of tension stiffening in the ﬁnal deﬂection calculations, the distribution factor ζ at time τk is obtained from Eq. 8.3: ζ = 1−

−32.8 −196

2 = 0.972

and the average curvatures at the supports of the column strip are obtained from Eq. 8.2. Instantaneous curvature due to Mvar : κuncr = −0.98×10−6 mm−1 ;κcr = −3.19×10−6 mm−1 ; and therefore κavge = −3.13×10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = −7.85×10−6 mm−1 ;κcr = −14.23×10−6 mm−1 ; and therefore κavge = −14.05×10−6 mm−1 . At mid-span The maximum in-service moment in the column strip at mid-span (due to wsus + wvar ) is 85 kNm and, from Section 5.3, the cracking moment at ﬁrst loading is 75.1 kNm and after all shrinkage is 56.0 kNm. The critical cross-section at mid-span will crack. The ﬁnal time-dependent curvature at mid-span caused by the moment due to the sustained load (Msus = 57.6 kNm) plus shrinkage and the short-term curvature caused by the moment due to the variable load (Mvar = 27.4 kNm) are next determined using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked section and Sections 7.2 and 7.3 for the cracked section. The distribution factor ζ at time τk is obtained from Eq. 8.3:

56.0 ζ = 1− 85

2 = 0.566

and the average curvatures at mid-span of the column strip are obtained from Eq. 8.2: Instantaneous curvature due to Mvar : κuncr = 0.44×10−6 mm−1 ;κcr = 2.79×10−6 mm−1 ; and therefore κavge = 1.77 ×10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = 3.81×10−6 mm−1 ;κcr = 11.71×10−6 mm−1 ; and therefore κavge = 8.28×10−6 mm−1 .

334 Members and structures Deﬂection The short-term deﬂection at mid-span of the column strip due to the variable loading is: 69502 (−3.13 + 10 × 1.77 + −3.13) × 10−6 = 5.8 mm 96

(vcx )var =

and the long-term deﬂection due to the sustained load and shrinkage is: 69502 (−14.05 + 10 × 8.28 − 14.05) × 10−6 = 27.5 mm 96

(vcx )sus =

The maximum total panel deﬂection at mid-span of the columns strip is therefore: (vcx )max = (vcx )var + (vcx )sus = 33.3 mm

Middle strip deﬂection (y-direction) The cracking moment for the middle strip at the support after all shrinkage has taken place is −58.4 kNm and at mid-span is 60.4 kNm, so the strip may suffer minor cracking at the support line (where from Table 8.6 the maximum in-service moment Msus+var = −66 kNm) but will be uncracked at mid-span (where Msus+var = 56 kNm). At the support At time τk : ζ = 1−

−58.4 −66

2 = 0.217

Due to Mvar : κuncr = −0.35 × 10−6 mm−1 ; κcr = −3.05 × 10−6 mm−1 ; and therefore κavge = −0.94 × 10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = −3.01 × 10−6 mm−1 ; κcr = −12.77 × 10−6 mm−1 ; and therefore κavge = −5.13 × 10−6 mm−1 . At mid-span Due to Mvar : κavge = κuncr = 0.30 × 10−6 mm−1 Due to Msus + shrinkage: κavge = κuncr = 2.58 × 10−6 mm−1 . Deﬂection The short-term deﬂection at mid-span of the middle strip due to the variable loading is: (vmy )var =

69502 (−0.94 + 10 × 0.30 − 0.94) × 10−6 = 0.6 mm 96

Members and structures

335

and the long-term deﬂection due to the sustained load and shrinkage is:

(vmy )sus =

69502 (−5.13 + 10 × 2.58 − 5.13) × 10−6 = 7.8 mm 96

The maximum total panel deﬂection at mid-span of the middle strip in the ydirection is: (vmy )max = (vmy )var + (vmy )sus = 8.4 mm

Panel deﬂection Finally, the maximum deﬂection at the mid-point of the panel is obtained from Eq. 8.16: vmax =

33.3 + 33.3 + 8.4 = 41.7 mm 2

8.5 Slender reinforced concrete columns 8.5.1 Discussion In most structural members, creep and shrinkage of concrete cause increases of deformation and redistribution of stresses, but do not affect strength. In some situations, however, the deformations caused by creep and shrinkage can lead to an increase in the loads on the structure and, therefore, a reduction in strength. A slender column under sustained, eccentric compression is such an example. Other examples include shallow concrete arches and domes. Consider the slender pin-ended column shown in Fig. 8.27. The column is subjected to a compressive force P applied at an initial eccentricity e0 . When P is ﬁrst applied at time τ0 , the column shortens and deﬂects laterally by an amount δ0 . The bending moment at each end of the column is Pe0 , but at the column mid-length, the moment is P(e0 + δ0 ). Therefore, the lateral deﬂection of the member causes an increase in the internal actions. For long columns, the secondary moment Pδ0 may be many times greater than the initial primary moment Pe0 and the load-carrying capacity is much less than that of a short column with the same cross-section. For very long columns, an instability failure may occur under relatively small compressive loads, i.e. buckling may occur before the strength of the cross-section at mid-length is reached. For reinforced concrete columns under sustained loads, the member suffers additional lateral deﬂection due to creep. This time-dependent deformation leads to additional bending in the member, which in turn causes the column to deﬂect still further. During a period of sustained loading, an additional deﬂection δ(t) will develop at the mid-length of the column. The gradual increase in the secondary moment with time P(δ0 + δ(t)) reduces the factor of safety and, for long columns, creep buckling may occur.

336 Members and structures P

P A

C

e0

(a) Initial geometry

P e0 A

e0

C

d0

C

P (b) At time t0

PDd(t) P d0 P e0

e0 d0 + Dd(t)

B

B P

P A

B P (c) At time t

P e0 (d) Bending moments

Figure 8.27 Displacements and moments in a slender pin-ended column.

In order to design slender reinforced concrete columns for the strength limit state, an accurate assessment of the creep deformation is necessary to ensure an adequate factor of safety. In the following section, an iterative computer-based procedure for the analysis of slender reinforced concrete columns is presented. 8.5.2 An iterative method of analysis To account for the geometric non-linearity associated with the secondary actions in a slender column (Pδ0 + Pδ(t)), as well as the material non-linearity associated with cracking, creep and shrinkage, an iterative solution procedure that uses the AEMM to include the time effects is described here. The analyses of cross-sections in the uncracked parts of the column are undertaken using the method described in Sections 5.3 and 6.2 (for short-term analysis) and Sections 5.4 and 6.3 (for long-term analysis), while for cross-sections in the cracked parts of the column, the analyses are undertaken in accordance with Section 7.2 (for short-term behaviour) and Section 7.3 (for time-dependent behaviour). Consider again the pin-ended column shown in Fig. 8.27. The iterative solution procedure involves the following steps: (i) The member is subjected initially to the axial load P and the primary moment Pe0 on every cross-section. The initial strain distributions and curvatures are calculated at the cross-sections at each end of the member (i.e. at A and B) and at the midlength (C). (ii) The lateral deﬂection of the member at the mid-length of the column, δ0 , is determined from the initial curvatures calculated in step (i). If a parabolic variation of curvature along the member is assumed, δ0 may be calculated using Eq. 8.1b. (iii) The additional increment of moment caused by δ0 at the mid-length of the columns (Pδ0 ) is added to the primary moment and the cross-section at C is re-analysed. The curvature at C is now larger than that calculated in step (i), and so too is the

Members and structures

337

lateral deﬂection δ1 at the mid-length of the column (re-calculated using Eq. 8.1b). The revised secondary moment (Pδ1 ) is added to the primary moment at C and the cross-section is again reanalysed. The procedure continues until the lateral displacement at C converges to δi after the ith iteration. The short-term response of the slender column is thus determined. The lateral deﬂection at C immediately after loading (δi ) is known, as is the stress and strain distributions on the cross-sections at A, B and C. If the member is very slender, convergence may not occur in step (iii) and a buckling instability may result. The secondary moment Pδ calculated during the iterative cycle, may cause cracking on a previously uncracked cross-section and therefore result in considerable loss of stiffness and an increase in the lateral displacement and secondary moment. The number of iterations required for convergence therefore depends on the slenderness of the member, the initial eccentricity and the tensile strength of the concrete. In step (iii), convergence may be deemed to occur when the additional lateral displacement calculated at mid-length during the ith iteration (δi – δi−1 ) is less than 0.001 of the lateral displacement δ0 caused by the primary moments and calculated in step (ii). With the behaviour immediately after loading at τ0 determined in step (iii), the time analysis commences: (iv) The time-dependent changes in strain and curvature at A, B and C are calculated using the previously speciﬁed time analyses. Initially, the internal actions at C (P and P(e0 + δi )) are assumed to remain constant with time. The change in the lateral displacement at C (δ0 ) caused by the change in curvature with time at each cross-section is calculated using Eq. 8.1b. This increase in displacement with time causes an additional increment of secondary moment Pδ0 to be applied gradually to the cross-section at C. This time-dependent secondary moment, in turn, produces additional lateral displacements and additional increments of secondary moment. An iterative procedure is again followed until the time-dependent lateral displacement converges to δ(t) (or until instability occurs). To model behaviour using the AEMM, the time-dependent increments of secondary moment, which in fact occur gradually, are applied to the age-adjusted transformed cross-section at mid-span. For initially cracked cross-sections, the depth to the neutral axis is assumed to remain constant with time. As was discussed in Section 7.3, this assumption, although not correct, is a reasonable compromise between accuracy and economy of solution. A more reﬁned analysis could be implemented to trace the development of time-dependent cracking using the SSM based on the iterative procedure outlined in Section 7.4.

Example 8.9 A pin-ended column with the cross-section shown in Fig. 8.28 is subjected to a constant sustained axial compressive load P = 500 kN acting at a constant eccentricity of e0 = 65 mm. The behaviour of the column is to be determined,

338 Members and structures both at ﬁrst loading τ0 and at time inﬁnity, for each of the following three column lengths: (i) L = 6000 mm; (ii) L = 7500 mm; and L = 9000 mm. Material properties are: Ec = 25,000 MPa; Es = 200,000 MPa; fc = 25 MPa; ft = 2.5 MPa; φ ∗ (τ0 ) = 2.5; fct = 2.5 MPa; φ ∗ (τ0 ) = 2.5; χ ∗ (τ0 ) = 0.65; and ∗ = 0. εsh 300

60

As = 900 mm2

P = 500 kN x

As = 900 mm2

180

65

60 y

Figure 8.28 Column section for Example 8.9 (all dimensions in mm).

Case (i): L = 6000 mm The initial stresses and strains on each cross-section due to the axial force P = 500 kN and the moment Pe0 = 32.5 kNm are calculated using the crosssectional analysis described in Section 5.3. In this case, the primary moment and axial force at each end and at mid-length are the same. On each cross-section, the compressive strain at the reference x-axis and curvature are εr,0 = −195 × 10−6 and κ0 = 1.673 × 10−6 mm−1 and the extreme ﬁbre concrete stresses are σtop = −11.15 MPa and σbot = +1.40 MPa. Since the tensile strength of the concrete is not exceeded, the member is uncracked. The lateral displacement at the column mid-length caused by the primary moment is obtained from Eq. 8.1b: δo =

60002 (1.673 + 10 × 1.673 + 1.673) = 7.53 mm 96

and the increment of secondary moment at the column mid-length Pδ0 = 3.76 kNm. This secondary moment is added to the primary moment and the cross-section at mid-length is re-analysed. The revised curvature at midlength is (κi )1 = 1.841 × 10−6 mm−1 and the revised displacement at mid-length is calculated using Eq. 8.1b is δ1 = 8.16 mm. The corresponding secondary moment is Pδ1 = 4.08 kNm. The revised secondary moment is added to the primary moment and the section at C is again re-analysed. The procedure continues for two more iterations until the lateral deﬂection converges to δi = 8.33 mm. The stress and strain distributions at mid-length are εr,0 = −195 × 10−6 ; κ0 = 1.887 × 10−6 mm−1 ; σtop = −11.95 MPa; and σbot = +2.20 MPa. The section at mid-length therefore remains uncracked.

Members and structures

339

For the time analysis, the cross-sections at each end and at the mid-length of the column are analysed using the procedure outlined in Section 5.4. Initially, the internal actions are assumed to remain constant. The change in the lateral displacement at mid-length caused by the change in curvature on each crosssection with time is δ0 = 14.23 mm. The secondary moment Pδ0 is applied to the age-adjusted transformed cross-section at mid-length, thus producing an additional increment of displacement and secondary moment. Convergence occurs after ﬁve iterations. The time-dependent change in displacement at the column mid-length is δi = 17.73 mm. The column therefore suffers a total mid-length lateral deﬂection of δi + δi = 26.06 mm. The initial and ﬁnal strain distributions and concrete stresses on the crosssections at each end and at the mid-length of the column are illustrated in Fig. 8.29. It is noted that the ﬁnal bottom ﬁbre tensile stress exceeds the tensile stress of the concrete indicating that cracking in the mid-length region of the column is likely to occur with time. −1216

−11.15 −7.86

−446

Initial Final

56 144 Strain (× 10−6)

0.9 1.4 Concrete stress (MPa)

(a) At each end of the column −1368

−478

−11.95 −9.62

Initial Final

88 428 Strain (× 10−6)

2.2 2.98 Concrete stress (MPa)

(b) At the mid-length of the column

Figure 8.29 Stresses and strains for case (i) of Example 8.9.

Case (ii): L = 7500 mm The stress and strain distributions at each end of the column are the same as those calculated in case (i). However, the increased column length results in larger lateral displacements and increased secondary moments. The secondary moments in this case are large enough to cause cracking at the mid-length of the column at initial loading. The initial and ﬁnal lateral displacements at the column mid-length in case (ii) are δi = 16.43 mm and δi + δ = 69.71 mm and the corresponding strains and stresses on the cross-section at mid-length are shown in Fig. 8.30a.

340 Members and structures

Case (iii): L = 9000 mm In this case, the initial column deﬂection at mid-length is δi = 30.03 mm and the initial states of stress and strain on the cross-section at the mid-point of the column are shown in Fig. 8.30b. As time progresses, additional secondary moments caused by creep become so large that convergence does not occur and the member buckles. For such a slender member, creep deformations result in a reduction of strength with time. −2043

−543

−14.68 −13.56 219.7

Initial Final 3.19 198 Strain (× 10−6)

1265 Concrete stress (MPa) (a) Case (ii)

−628

−15.69 Initial 194.6

Creep buckling occurs with time! 0

340 Strain (× 10−6)

Concrete stress (MPa)

(b) Case (iii)

Figure 8.30 Stresses and strains at the column mid-length for Example 8.9.

8.6 Temperature effects 8.6.1 Introduction A uniform or linearly varying temperature distribution through the depth of a statically determinate homogeneous member causes the member to deform, but no stress is produced on any cross-section. In practice, however, temperature rarely varies linearly through the depth of a member and members are usually unable to accommodate the deformation caused by temperature change without some restraining forces developing at the supports. Because plane sections tend to remain plane, a non-linear temperature gradient produces internal, self-equilibrating eigenstresses, as illustrated in Fig. 8.31. The free expansion (or contraction) of each concrete ﬁbre is restrained by the adjacent ﬁbres resulting in the internal stress distribution shown. A similar distribution of selfequilibrating internal stress is produced by non-linear shrinkage and was discussed in Section 1.3.3 and illustrated in Fig. 1.13. Usually design engineers are concerned with temperature changes applied over a short time period. If the temperature gradient is sustained for a period of time, the

Members and structures

341

To Elastic + creep strain

s(y)

Unrestrained temperature strain = αT(y)

T(y)

Total strain

(a) Temperature change

(b) Strain

(c) Self-equilibrating stress

Figure 8.31 Effects of non-linear temperature distribution on cross-sectional response.

internal stresses induced by temperature are relieved, to some extent, by creep. If necessary, a time analysis using the AEMM can be used to determine the variation of cross-sectional behaviour with time. In a statically indeterminate member, the displacement at the member’s ends caused by the axial deformation and curvature induced by temperature may not be free to occur. Reactions develop at the supports and internal actions are induced at each cross-section of the member. The stresses resulting from these secondary actions can be large and must be calculated and added to the stresses illustrated in Fig. 8.31, if the total stresses on a cross-section of a statically indeterminate member are required. The determination of these continuity stresses is discussed in Section 8.6.4. 8.6.2 Temperature distributions Temperature variations caused by solar radiation in bridge decks, for example, can produce stress levels that are of similar magnitude to those produced by the gravity loads, even if the structure is statically determinate. In the design of such structures, an analysis to determine the effects of temperature often plays an important part. Design codes provide guidance on temperature gradients that should be considered for particular structural applications. For example, typical temperature proﬁles to be used in the design of composite concrete-concrete bridges are shown in Fig. 8.32 and are based on the Australian speciﬁcations (Refs 21 and 22). 8.6.3 Temperature analysis of cross-sections In this section, the short-term analysis of a cross-section subjected to an arbitrary nonlinear temperature variation at time τ0 is presented. The overall method of analysis is similar to that presented in Sections 5.3–5.7, except that a thermal-induced strain is included in the constitutive relationship of each constituent material. For a reinforced or prestressed concrete cross-section with mc concrete components, ms layers of non-prestressed reinforcement and mp layers of prestressing tendons, the constitutive relationships are: σc(i),0 = Ec(i),0 ε0 − εc(i),T

(8.17a)

342 Members and structures Max Dd = 300 mm y

Ttop

0.4Ttop

24°C

300

300 300

D

Ttop +3 T(°C) Dd

6°C

T(y) = Ttop + 3 − 0.05y Temperature profile across deck slabs over closed box cells (shaded area)

D

T(y) = Ttop 1− 200

(a) Concrete deck on girder (Ref. 21)

y 5 1200

5 if soffit is within 8 m of ground 0 if over water y (mm)

(b) Box girder bridge deck (Ref. 22)

Figure 8.32 Temperature gradients for concrete box girders (Refs 21–22).

σs(i),0 = Es(i) ε0 − εs(i),T σp(i),0 = Ep(i) ε0 + εp(i),init − εp(i),T

(8.17b) (8.17c)

where εc(i),T , εs(i),T and εp(i),T are the thermal-induced strains in the concrete, nonprestressed reinforcement and prestressing tendons, respectively, and are determined from: εc(i),T = αc(i),T T (y)

(8.18a)

εs(i),T = αs(i),T T (y)

(8.18b)

εp(i),T = αp(i),T T (y)

(8.18c)

in which T(y) is the temperature distribution on the cross-section as a function of distance y from the reference axis, and αc(i),T , αs(i),T and αp(i),T are the coefﬁcients of thermal expansion for the concrete, non-prestressed reinforcement and prestressing tendons, respectively. The contributions to the internal axial force on the cross-section of the constituent materials at time τ0 after the temperature change are: Nc,0 =

mc

σc(i),0 dA =

i=1A c(i)

−

mc i=1A c(i)

mc

Ac(i) Ec(i),0 εr,0 +

i=1

Ec(i),0 εc(i),T dA

mc

Bc(i) Ec(i),0 κ0

i=1

(8.19a)

Members and structures Ns,0 =

ms

As(i) Es(i) εr,0 +

i=1

ms

ys(i) As(i) Es(i) κ0 −

i=1

ms

As(i) Es(i) εs(i),T

343

(8.19b)

i=1

mp mp mp Np,0 = Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(j) Ep(i) εp(i),init i=1

i=1

i=1

mp

−

Ap(i) Ep(i) εp(i),T

(8.19c)

i=1

Combining these contributions, the internal axial force and bending moment resisted by the whole cross-section are: mp Ni,0 = Nc,0 +Ns,0 +Np,0 = RA,0 εr,0 +RB,0 κ0 + Ap(j) Ep(j) εp(j),init −NT,0 j=1

(8.20a) mp

Mi,0 = Mc,0 +Ms,0 +Mp,0 = RB,0 εr,0 +RI,0 κ0 +

yp(i) Ap(i) Ep(i) εp(i),init −MT,0 i=1

(8.20b) where the cross-sectional rigidities at time τ0 , i.e. RA,0 , RB,0 and RI,0 , have already been deﬁned in Eqs 5.72, and NT,0 and MT,0 are the equivalent actions required to produce the same deformation as the temperature change if each material was unrestrained and are given by: NT,0 =

mc

Ec(i),0 εc(i),T dA +

i=1A c(i)

mp ms As(i) Es(i) εs(i),T + Ap(i) Ep(i) εp(i),T i=1

i=1

(8.21a) MT,0 =

mc

yEc(i),0 εc(i),T dA +

i=1A c(i)

ms ys(i) As(i) Es(i) εs(i),T i=1

mp yp(i) Ap(i) Ep(i) εp(i),T +

(8.21b)

i=1

Substituting Ni,0 and Mi,0 (Eqs 8.20) into Eqs 5.2, the equilibrium equations may be expressed as: re,0 = D0 ε0 + fp,init − fT

(8.22)

and solving Eq. 8.22 gives the unknown strain variables ε0 : ε0 = D−1 re,0 − fp,init + fT = F0 re,0 − fp,init + fT 0

(8.23)

344 Members and structures where ε0 , re,0 , D0 , F0 and f p,init are all deﬁned in Eqs 5.71 and f T is given by:

NT,0 fT = MT,0

(8.24)

Evaluation of the integral expressing the thermal response of the concrete can be carried out numerically or in closed form when the temperature variation is speciﬁed with a known function.

Example 8.10 The stress and strain distributions on the section shown in Fig. 8.33a caused by the temperature gradient shown in Fig. 8.33b are to be calculated. The cross-section is of a statically determinate beam and the rise in temperature is applied over a short time period. Because temperature rises are associated with expansion, they are here taken to be positive. The coefﬁcient of thermal expansion for both concrete and steel is αc = αs = 10 × 10−6 /o C and the prestressing steel is bonded to the surrounding concrete. Take Ec = 30,000 MPa and Es = Ep = 200,000 MPa. 400 200

20°C 100

200

200

As2 = 400 mm2 200

x

600 2

Ap = 2000 mm

y

2°C

300

As2 = 1240 mm2 200 100

200

(a) Cross-section

20

300 0

T(y)

5°C

eT = αT(y)

50

(b) Temperature gradient

(c) Free temperature induced strain

Figure 8.33 Section details and temperature gradient for Example 8.9.

The free temperature strain εT = αT(y) is shown in Fig. 8.33c and the equivalent actions NT,0 in each material are: NTc,0 =

mc

Ec(i),0 εc(i),T dA = [400 × 200 ×

i=1A c(i)

+ 200 × 300 ×

(200 − 20) + 400 × 200 × 20 2

50 20 + 400 × 200 × − 400 × 110 2 2

− 1240 × 25] × 10−6 × 30,000 = 339.8 kN

Members and structures NTs,0 =

345

ms As(i) Es(i) εs(i),T = [400 × 110 + 1240 × 25] × 10−6 × 200,000 i=1

= 15.0 kN mp NTp,0 = Ap(i) Ep(i) εp(i),T = [2000 × 200,000 × 0] = 0 i=1

and the moments of these forces about the centroidal axis of the section are: MTc,0 =

mc

yEc(i),0 εc(i),T dA = [400 × 200 ×

i=1A c(i)

(200 − 20) ˙ × (−433.3) 2

+ 400 × 200 × 20 × (−400) + 200 × 300 × + 400 × 200 ×

20 × (−200) 2

50 × 433.3 − 400 × 110 × (−400) 2

− 1240 × 25 × 400] × 10−6 × 30,000 = −90.25 kNm MTs,0 =

ms ys(i) As(i) Es(i) εs(i),T = [400 × 110 × (−400) i=1

+ 1240 × 25 × 400] × 10−6 × 200,000 = −1.04 kNm mp yp(i) Ap(i) Ep(i) εp(i),T = [300 × 2000 × 200,000 × 0] = 0 NTp,0 = i=1

From Eqs 8.21: NT,0 = NTc,0 + NTs,0 + NTp,0 = 354.8 kN MT,0 = MTc,0 + MTs,0 + MTp,0 = −90.25 − 1.04 = −91.29 kNm The rigidities of this cross-section are obtained from Eqs 5.72 as RA,0 = 9.02 × 109 N, RB,0 = 15.91 × 1010 Nmm, RI,0 = 9.67 × 104 Nmm2 , and with the F0 matrix for this cross-section calculated using Eq. 5.71b, the strain matrix for the otherwise unloaded cross-section is determined using Eq. 8.23:

−1.829 × 10−14 1.112 × 10−10 ε0 = F0 fT = −14 −1.829 × 10 1.037 × 10−15 41.1 × 10−6 = −0.1012 × 10−6 mm−1

354.8 × 103 −91.29 × 106

346 Members and structures The top (y = −500 mm) and bottom (y = +500 mm) ﬁbre strains are: ε0,top = 41.1 × 10−6 + (−500) × (−0.1012 × 10−6 ) = 91.7 × 10−6 ε0,bot = 41.1 × 10−6 + 500 × (−0.1012 × 10−6 ) = −9.5 × 10−6 The temperature-induced changes of stress in the concrete are determined from Eq. 8.17a as follows: At y = −500 mm: σ c,0 = 30,000[41.1 + (−500) × (−0.1012) − 200] × 10−6 = −3.25 MPa At y = −300 mm: σc,0 = 30,000[41.1 + (−300) × (−0.1012) − 20] × 10−6 = 1.54 MPa At y = 0 mm: σc,0 = 30,000[41.1 + (0) × (−0.1012) − 0] × 10−6 = 1.23 MPa At y = +300 mm: σc,0 = 30,000[41.4 + (300) × (−0.1012) − 0] × 10−6 = 0.32 MPa At y = +500 mm: σc,0 = 30,000[41.4 + (500) × (−0.1012) − 50] × 10−6 = −1.79 MPa From Eqs 8.17b and c: σs(1) = 200,000[41.4 + (−400) × (−0.1012) − 110] × 10−6 = −5.68 MPa σs(2) = 200,000[41.4 + (400) × (−0.1012) − 25] × 10−6 = −4.88 MPa σp = 200,000[41.4 + (300) × (−0.1012) − 0] × 10−6 = −2.15 MPa The temperature-induced strains and eigenstresses on the concrete section are shown in Fig. 8.34. 91.7

200

−3.25

−

20

1.54

Free temperature strain, eT +

1.23

Actual strain, e0

0.32 − −9.5

50

Strain (×10−6)

−1.79

Concrete stress (MPa)

Figure 8.34 Temperature-induced stress and strain in Example 8.10.

Members and structures

347

8.6.4 Temperature effects in members and structures The temperature-induced strains on individual cross-sections cause axial deformation and rotation of members and structures. In statically indeterminate members, the displacement caused by temperature changes may not be free to occur, and restraining forces may develop at the supports. The stresses and deformations caused by these restraining forces must be calculated and added to the temperature-induced eigenstresses in order to obtain the total effect of temperature. The redundant forces caused by restraint to temperature can be determined using exactly the same procedure as outlined in Section 8.3.2.

Example 8.11 A beam with cross-section shown in Fig. 8.33a is subjected to the temperature gradient of Fig. 8.33b applied over its entire length in an eight-hour period. If the beam was statically determinate, the temperature-induced stresses and strains on the cross-section were calculated in Example 8.10 and illustrated in Fig. 8.34. From Example 8.10, the temperature-induced strain at the reference axis (at the mid-depth of the cross-section) and the curvature on each cross-section of the beam are: εr,0 = 41.1 × 10−6 and κ0 = −0.1012 × 10−6 mm−1 .

(a) The beam is uncracked throughout and simply supported over a span of 14 m The displacement of the beam (idealised in Fig. 8.35a) is to be determined. The axial deformation of the member is: eAB = εr,0 L = 41.1 × 10−6 × 14,000 = 0.58 mm (elongation) and the deﬂection at mid-span is calculated using Eq. 8.1b: vC =

14,0002 12 × (−0.1012) × 10−6 = −2.48 mm 96 θA

A

vC

C L = 14,000 mm

eAB B

(a) Simply-supported beam MA

VA

VB (b) Redundant reactions if end A is fixed

Figure 8.35 Temperature-induced deformations and reactions in Example 8.11.

348 Members and structures From Eq. 3.7b, the slope at each end of the beam is: θA = θB =

14,000 3 × (−0.1012 × 10−6 ) = −0.708 × 10−3 rad 6

(b) The support at A is ﬁxed, so that θA is prevented If the rotation at A cannot occur, the temperature gradient will induce the reactions shown in Fig. 8.35b at the supports. For this analysis, the moment at A is taken to be the redundant, RR = MA , and the deformation of the primary structure at the release is: uA = θA = −0.708 × 10−3 Due to a unit moment applied at A, the rotation at A is f11 and the reactions at the supports of the primary beam are RPR , where: L f11 = 3Ec I

and RPR =

2 ! VA = −1 L 2 VB = +1 L

For this beam, Ec = 30,000 MPa and the second moment of are of the transformed cross-section about its centroidal axis is equal to I = 31,040 ×106 mm4 . Therefore: ¯f11 =

14,000 = 5.01 × 10−12 3 × 30,000 × 31,040 × 10−6

From Eq. 8.5, the redundant moment at A is:

RR = MA = −

−0.708 × 10−3 = 141.3 kNm 5.01 × 10−12

and the other reactions of the statically indeterminate beam are determined from statics: VB =

MA 141.3 × 106 = = 10.09 kN L 14,000

and VA = −VB = −10.09 kN

The temperature-induced eigenstresses at the support A were calculated in Example 8.10 and are reproduced in Fig. 8.36a. In Fig. 8.36b, the continuity stresses in the concrete caused by the redundant moment MA are also shown. The resultant temperature-induced stresses are obtained by summing the eigenstresses and the continuity stresses and are illustrated in Fig. 8.36c.

Members and structures −3.25

−5.55

−2.30

−

− 0.16

−

1.54 + 1.23

349

+

1.22

= +

0.32 − −1.79 (a) Eigenstresses

1.66

+ +2.25 (b) Continuity stresses

0.46 (c) Resultant stresses

Figure 8.36 Temperature-induced concrete stresses at ﬁxed support at A in Example 8.11.

8.7 Concluding remarks The techniques described and illustrated in this chapter may be extended readily to include a wide range of additional structural applications. The procedures are not daunting and require little more than an elementary background in mechanics and structural analysis. An analysis for the effects of creep and shrinkage on the behaviour of concrete structures allows the structural design engineer to better predict and control inservice performance. But perhaps of greater importance, it provides a clear picture of the interaction between concrete and reinforcement at service loads and a better understanding of why concrete structures behave as they do.

8.8 References 1. British Standards Institution (2004). Eurocode 2: Design of Concrete Structures – part 1-1: General rules and rules for buildings BS EN 1992-1-1: 2004. European Committee for Standardization, Brussels. 2. Ghali, A. and Neville, A.M. (1978). Structural Analysis – A Uniﬁed Classical and Matrix Approach. Chapman and Hall, London. 3. Hall, A.S. and Kabaila, A.P. (1977). Basic Concepts of Structural Analysis. Pitman Publishing, London. 4. Mayer, H. and Rüsch, H. (1967). Building Damage Caused by Deﬂection of Reinforced Concrete Building Components. Technical Translation 1412, National Research Council Ottawa, Canada (Deutscher Auschuss für Stahlbeton, Heft 193, Berlin, West Germany). 5. Sbarounis, J.A. (1984). Multi-storey ﬂat plat buildings – measured and computed one-year deﬂections. Concrete International, 6(8), 31–35. 6. Jokinen, E.P. and Scanlon, A. (1985). Field measured two-way slab deﬂections. CSCE Annual Conference, Saskatoon, Canada, May. 7. Gilbert, R.I. and Guo, X.H. (2005). Time-dependent deﬂection and deformation of reinforced concrete ﬂat slabs – an experimental study. ACI Structural Journal, 102(3), 363–373.

350 Members and structures 8. Timoshenko, S. and Woinowsky-Krieger, S. (1959). Theory of Plates and Shells. McGrawHill Book Co., New York. 9. Marsh, C.F. (1904). Reinforced Concrete. D. Van Nostrand Co., New York. 10. Ewell, W.W., Okuba, S. and Abrams, J.I. (1952). Deﬂections in gridworks and slabs. Transactions, ASCE, 117, p. 869. 11. Furr, W.L. (1959). Numerical method for approximate analysis of building slabs. ACI Journal, 31(6), 511. 12. Vanderbilt, M.D., Sozen, M.A. and Siess, C.P (1963). Deﬂections of Reinforced Concrete Floor Slabs. Structural Research Series No. 263, Department of Civil Engineering, University of Illinois, April. 13. Rangan, B.V. (1976). Prediction of long-term deﬂections of ﬂat plates and slabs. ACI Journal, 73(4), 223–226. 14. Nilson. A.H. and Walters, D.B. (1975). Deﬂection of two-way ﬂoor systems by the equivalent frame method. ACI Journal, 72(5), 210–218. 15. Gilbert, R.I. (1985). Deﬂection control of slabs using allowable span to depth ratios. ACI Journal, 82(1), 67–72. 16. Scanlon, A. and Murray, D.W. (1974). Time-dependent reinforced concrete slab deﬂections. Journal of the Structural Division, ASCE, 100, 1911–1924. 17. Gilbert, R.I. (1979). Time-Dependent Behaviour of Structural Concrete Slabs. PhD Thesis, University of New South Wales, pp 361. 18. Chong, K.T., Foster, S.J. and Gilbert, R.I. (2008). Time-dependent modelling of RC structures using the cracked membrane model and solidiﬁcation theory. Computers and Structures, 86(11–12), 1305–1317. 19. Nilson, A.H. and Walters, D.B. (1975). Deﬂection of two-way ﬂoor systems by the equivalent frame method. ACI Journal, 72(5), 210–218. 20. American Concrete Institute (2008). Building Code Requirements for Reinforced Concrete ACI 318M-08 and Commentary. ACI Committee 318, Michigan, USA. 21. National Association of State Road Authorities (1992). NAASRA – Bridge design speciﬁcation. Sydney. 22. Standards Australia (2004). Bridge Design Part 2: Design Loads AS5100.2-2004. Sydney.

9

Stiffness method and ﬁnite-element modelling

9.1 Introduction The analysis of members and frames is commonly carried out in design ofﬁces using commercial software based on either the stiffness method or the ﬁnite-element approach. This chapter outlines how these methods can be used for the long-term analyses of concrete structures, accounting for the effects of creep and shrinkage. The solution procedures required for the methods are well established (Refs 1–3) and only a brief overview of them is provided here. Throughout the chapter frequent reference is made to Appendix A, where the detailed derivations required to establish the proposed approaches are outlined. Worked examples are also presented to better illustrate the methods.

9.2 Overview of the stiffness method The stiffness method of analysis, also referred to as the displacement method, is a matrix method for the analysis of complex structural systems using computers. A beam or frame is discretised into a number of line elements, referred to as stiffness elements, connected at their ends by nodes. A typical two-dimensional six degree of freedom (6 DOF) frame element of length L is illustrated in Fig. 9.1, where the three possible displacement components at each end node and the three corresponding nodal actions are shown. The overall structural response is evaluated by combining the contribution of each single element in resisting the applied loads or deformations. This approach relies on the fact that, for each element, it is possible to establish a stiffness relationship between nodal actions and nodal displacements, i.e.: p = ke u

(9.1)

where p and u are the nodal actions and displacements of an element, and ke is the element stiffness matrix. For any particular element, this relationship is expressed in its particular coordinate system (usually referred to as the local or member

352 Stiffness method and ﬁnite-element modelling coordinate system). For example, for the 6 DOF frame element of Fig. 9.1, the stiffness matrix is derived in Appendix A as Eq. A.51 and is reproduced here as: ⎡

RA ⎢ ⎢ L ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ RB ⎢− ⎢ L ke = ⎢ ⎢ ⎢ RA ⎢− ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎣ R B L

0 12 α1 L 3 6 α1 L 2 0 −

12 α1 L3

6 α1 L 2

RB − L 6 α1 L2 R2 4 + B α 1 L RA L

RA − L

RB L 6 − α1 L2 R2 2 − B α 1 L RA L

RA L

0

0

12 α 1 L3

0

0

−

12 α1 L 3

RB L

−

6 α1 L 2

−

RB L

−

6 α1 L 2

⎤ RB ⎥ ⎥ L ⎥ ⎥ 6 ⎥ ⎥ α1 L2 ⎥ ⎥ R2B ⎥ 2 ⎥ − α1 L R A L ⎥ ⎥ ⎥ ⎥ RB ⎥ − ⎥ L ⎥ ⎥ 6 ⎥ − ⎥ α1 L 2 ⎥ ⎥ R2B ⎦ 4 + α1 L R A L

(9.2a)

and the nodal actions and displacements shown in Fig. 9.1 are: ⎡

⎤ NL ⎢ ⎥ ⎢ SL ⎥ ⎢ ⎥ ⎢ ML ⎥ ⎢ ⎥ p=⎢ ⎥ ⎢ NR ⎥ ⎢ ⎥ ⎣ SR ⎦ MR ⎡ ⎤ uL ⎢ ⎥ ⎢ vL ⎥ ⎢ ⎥ ⎢ θL ⎥ ⎥ u=⎢ ⎢u ⎥ ⎢ R⎥ ⎢ ⎥ ⎣ vR ⎦ θR

(9.2b)

(9.2c)

The rigidities RA , RB and RI have been introduced in Chapters 5 and 7 for different types of cross-sections, and the coefﬁcients α0 and α1 are calculated from the rigidities using Eqs A.50a and b. The subscripts ‘L’ and ‘R’ on the nodal loads and displacements denote the left (at z = 0) and right (at z = L) member ends, respectively, when looking at the element with the z-axis horizontal and pointing towards the right. In the proposed formulation, the coordinate system is illustrated in Fig. 9.2 for a typical reinforced concrete member. To remain consistent with the coordinate systems adopted in previous chapters, rotations are assumed to be positive when clockwise and transverse displacements are positive when in the direction of the y-axis. In a real structure, members may have different orientations (with different local coordinate systems). It is therefore convenient to introduce a global coordinate system to be used for the whole structure. The load and displacement vectors for a particular

Stiffness method and ﬁnite-element modelling 353 qR

MR

uR

SR

vR uL

NL

L z

vL

qL

NR

ML

L SL

z

(b) Nodal actions

(a) Nodal displacements

Figure 9.1 Freedoms of the 6 DOF frame element.

z

L x y

Figure 9.2 Coordinate system adopted for the member analysis.

element (deﬁned in local coordinates in Eqs 9.2b and c, respectively) can be expressed in global coordinates by carrying out the following transformations: u = TUe

(9.3a)

Pe = TT p

(9.3b)

where Pe represents the load vector in global coordinates, Ue is the vector of nodal displacements in global coordinates, and the transformation matrix T is given by: ⎡

c s 0 0 0 ⎢ ⎢−s c 0 0 0 ⎢ ⎢ ⎢0 0 1 0 0 T=⎢ ⎢0 0 0 c s ⎢ ⎢ ⎣ 0 0 0 −s c 0 0 0 0 0

⎤ 0 ⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥ 0⎥ ⎥ ⎥ 0⎦ 1

(9.4)

where c and s are, respectively, the cosine and the sine of the angle between the global and local coordinate systems (measured clockwise from the global system).

354 Stiffness method and ﬁnite-element modelling Substituting Eqs 9.3 into Eq. 9.1 gives the stiffness relationship of a particular element expressed in global coordinates: Pe = Ke Ue

(9.5)

where Ke is the stiffness matrix of the element in global coordinates given by: K e = T T ke T

(9.6)

The stiffness relationship for the whole structure is then obtained by assembling the contribution of each element and can be expressed as: P = KU

(9.7)

where K is the structural stiffness matrix, while P and U are, respectively, the vectors of nodal actions and displacements for the whole structure expressed in the global coordinate system. Equation 9.7 is readily solved for the unknown displacements and reactions. For illustrative purposes, Eq. 9.7 can be re-written in terms of the known and unknown displacements (UK and UU ) and known and unknown actions (PK and PU ) as follows: K11 K12 UU PK = (9.8) PU K21 K22 UK The unknown displacements and actions are determined as follows: −1 UU = K11 (PK − K12 UK )

(9.9a)

PU = K21 UU + K22 UK

(9.9b)

9.3 Member loads Distributed member loads can be considered in the analysis by introducing particular sets of nodal actions that produce equivalent effects to the original distributed loads and, for this reason, are usually referred to as equivalent nodal loads. These correspond to the opposite of the reactions that would occur at the end of a loaded stiffness element if its ends were assumed to be ﬁxed. Different sets of equivalent nodal loads have been derived in Appendix A. For example, in the case of uniform longitudinal and transverse distributed loads (referred to as n and p, respectively, in Fig. 9.3), the end reactions of a ﬁxed ended member pF.m are given in Eq. A.52 (reproduced here for ease of reference): ⎡ ⎤ ⎡ ⎤ 0 −L/2 ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ α3 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢Lα3 /2⎥ (9.10) pF.m = ⎢ ⎥ p+⎢ ⎥n ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ −L/2 ⎦ ⎣ α3 ⎦ L2 /12 Lα3 /2

Stiffness method and ﬁnite-element modelling 355 p NL ML

NR SL

n

SR

MR

Figure 9.3 Free body diagram of a frame element highlighting uniformly distributed vertical and horizontal member loads n and p.

The subscript ‘m’ indicates that the reactions relate to member loads, while the subscript ‘F’ indicates that these actions have been determined assuming both ends of the element are fully ﬁxed. The term α3 is the ratio of the cross-sectional rigidities RB and RA and is deﬁned in Eq. A.50d. The equivalent nodal loads for inclusion in the stiffness analysis are the opposite of these reactions (i.e. −pF.m ). The unknown displacements and reactions of the structure are obtained from Eqs 9.9 after the nodal loads from all elements are assembled. The actions on each element (depicted in Fig. 9.1b) can be calculated by adding the forces and moments caused by the calculated displacements (= ku) to the ﬁxed-end reactions speciﬁed in Eq. 9.10 as: p = ku + pF.m

(9.11)

Based on the Euler–Bernoulli beam assumptions, the displacements at any point along the length of an element are given by: z4 z3 z2 4 + C1 + C 2 + C 3 z + C 24 6 2 z2 z3 6 5 z + C +C u = α2 p + α3 C 1 + α4 n 6 2 v = α1 p

(9.12a) (9.12b)

where these equations are derived in Appendix A as Eqs A.53. The terms α1 , α2 , α3 and α4 are calculated from the cross-sectional rigidities and are given in Eqs A.50b–e. 1 to C 6 are obtained by specifying the appropriate The constants of integration C boundary conditions and are expressed in terms of the nodal (element) displacements and applied member loads in Eqs A.54. The expressions describing the variation of the axial strain (measured at the level of the x-axis) and curvature along the member length can be obtained by differentiating Eqs 9.12: u = α2 p

z2 5 + α3 C1 + α4 n z + C 2

(9.13a)

v = α1 p

z2 2 + C1 z + C 2

(9.13b)

356 Stiffness method and ﬁnite-element modelling For example, these expressions can be used to evaluate the internal axial force and moment resisted by the concrete (Eqs A.56 and A.58) which will become useful in the following sections dealing with time effects: Nc = Ac Ec u − Bc Ec v = ac0 + ac1 z + ac2 z2

(9.14a)

Mc = Bc Ec u − Ic Ec v = bc0 + bc1 z + bc2 z2

(9.14b)

The concrete cross-sectional properties have been deﬁned in Chapter 5, while the use of the parabolic polynomial to describe the variation of both Nc and Mc is justiﬁed in Appendix A for the derivation of Eqs A.56 and A.58. The coefﬁcients of the polynomials (ac0 , ac1 , ac2 , bc0 , bc1 , bc2 ) are given in Appendix A (Eqs A.57 and A.59). In the following example, a simple beam subdivided into two elements is considered for illustrative purposes only. Clearly, the method is more applicable for more complex structures.

Example 9.1 The instantaneous mid-span deﬂection of the simply-supported beam shown in Fig. 9.4 is to be determined using the stiffness method. The beam is subjected to the uniformly distributed transverse load and the axial point load shown. The set of external actions reproduces the loading condition of Example 5.1 at midspan of the member. The analysis is carried out using two stiffness elements of equal length numbered 1 and 2, respectively, as shown in Fig. 9.4. The geometry and material properties of the cross-section are as speciﬁed in Example 5.1 (including the use of the x-axis located at 200 mm below the top ﬁbre of the cross-section). The member actions for both elements are to be calculated, as are all the coefﬁcients necessary to deﬁne the expressions for the strain and for the internal actions resisted by the concrete along each element. 4 kN/m 30 kN 1

B

2

A 5m

5m

C

Figure 9.4 Loading, support conditions and discretisation for Example 9.1.

All units utilised in the solutions are in mm and N. For clarity, units are not displayed next to the terms in large matrices in the following solution. An additional subscript ‘(1)’ or ‘(2)’ is used to specify whether a variable is calculated for elements 1 or 2, respectively. Where variables are identical for both elements, the subscript might be omitted for ease of notation. This is usually the case for the cross-sectional rigidities and material properties that are identical for both elements. The freedoms for the problem are numbered in Fig. 9.5, where the lower numbers are used for the unrestrained freedoms. This numbering strategy is particularly useful for hand calculation as it leads to the partitioning introduced

Stiffness method and ﬁnite-element modelling 357 in Eqs 9.8. Also for this particular example, with the numbering proposed in Fig. 9.5, global and local coordinates coincide and there is no need to include transformations between the two coordinate systems in the solution, such as those described in Eqs 9.3 and 9.6.

1

A 8

7 1

2

B 3

2 4

C 9

5 6

Figure 9.5 Freedom numbering for Example 9.1.

Considering that freedoms 7, 8 and 9 are restrained by the pinned and roller supports, their displacements are known, while the displacements along the remaining freedoms are unknown. Therefore: T T T UK = U7 U8 U9 = 0 0 0 and UU = U1 U2 U3 U4 U5 U6 The unknown reactions are collected in PU : PU = P7

P8

P9

T

From Example 5.1, the instantaneous cross-section rigidities are: RA = 4923 × 106 N RB = 543.9 × 109 Nmm RI = 221.0 × 1012 Nmm2 and from Eqs A.50: α0 = R1 RA − R2B = 792.3 × 1021 N2 mm2 α1 =

RA = 6.214 × 10−15 N−1 mm−2 α0

α2 =

RB = 686.5 × 10−15 N−1 mm−1 α0

α3 =

RB = 110.5 mm RA

α4 = −

1 = −203.1 × 10−12 N−1 RA

358 Stiffness method and ﬁnite-element modelling The stiffness matrices for elements 1 and 2 are identical (as both possess the same geometric and cross-sectional properties) and are given by Eq. 9.2a: ⎡ ⎤ 984.7 × 103 0 −108.8 × 106 −984.7 × 103 0 108.8 × 106 ⎢ ⎥ ⎢ ⎥ ⎢ 15.45 × 103 38.62 × 106 0 −15.45 × 103 38.62 × 106 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ 9 6 6 9 140.7 × 10 108.8 × 10 −38.62 × 10 52.35 × 10 ⎥ ⎢ ⎥ k=⎢ ⎥ ⎥ ⎢ 3 6 ⎢ 984.7 × 10 0 −108.8 × 10 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ sym 15.45 × 103 −38.62 × 106 ⎥ ⎣ ⎦ 140.7 × 109

The ﬁxed end forces on each element due to the transverse load p = 4 N/mm are obtained from Eq. 9.10: ⎤ 0 ⎥ ⎢ ⎢ L⎥ ⎢− ⎥ ⎢ 2 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ L2 ⎥ ⎢− ⎥ ⎢ 12 ⎥ ⎥ pF.m(1) = pF.m(2) = ⎢ ⎥ ⎢ ⎢ 0 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ L⎥ ⎢− ⎥ ⎢ 2 ⎥ ⎥ ⎢ ⎣ L2 ⎦ 12

⎡

⎡

⎤

⎢ ⎥ 0N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢−8.3 × 106 Nmm⎥ ⎢ ⎥ p=⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎣ ⎦ 8.3 × 106 Nmm

Assembling the contribution of the two elements into the stiffness matrix of the structure enables the determination of the various sub-matrices of K given in Eq. 9.8: ⎡ ⎤ 140.7 × 109 108.8 × 106 −38.62 × 106 52.35 × 109 0 0 ⎢ ⎥ ⎢ ⎥ ⎢ 1.969 × 106 0 −217.6 × 106 −984.7 × 103 108.8 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 30.89 × 103 0 0 38.62 × 106 ⎥ ⎢ ⎥ K11 = ⎢ ⎥ 9 6 9 ⎥ ⎢ 281.5 × 10 108.8 × 10 52.35 × 10 ⎢ ⎥ ⎢ ⎥ 3 6⎥ ⎢ sym 984.7 × 10 −108.8 × 10 ⎣ ⎦

⎡

−108.8 × 106 ⎢ ⎢−984.7 × 103 ⎢ ⎢ 0 ⎢ K12 = ⎢ ⎢ 108.8 × 106 ⎢ ⎢ 0 ⎣ 0

38.62 × 106 0 −15.45 × 103 38.62 × 106 0 0

0

⎤

⎥ ⎥ ⎥ ⎥ −15.45 × 103 ⎥ ⎥ −38.62 × 106 ⎥ ⎥ ⎥ 0 ⎦ 6 −38.62 × 10 0

140.7 × 109

⎡ ⎢ K22 = ⎣

984.7 × 103

Stiffness method and ﬁnite-element modelling 359 ⎤ 0 0 ⎥ ⎦ 15.45 × 103 0 15.45 × 103

sym T K21 = K12

Assembling the load vector for the whole structure (including the axial load of −30 kN applied at freedom 5) produces: ⎡

⎤ 8.3 × 106 Nmm ⎢ ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢ 20 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 Nmm ⎢ ⎥ ⎢ 3 P = ⎢ −30 × 10 N ⎥ ⎥ ⎢ ⎥ ⎢−8.3 × 106 Nmm⎥ ⎢ ⎥ ⎢ ⎥ P7 ⎢ ⎥ ⎢ ⎥ 3 ⎣ P8 + 10 × 10 N ⎦ P9 + 10 × 103 N Unknown displacements UU and reactions PU are then calculated using Eqs 9.9: ⎡

1.138 × 10−3

⎤

⎢ ⎥ ⎢−156.2 × 10−3 mm⎥ ⎢ ⎥ ⎢ ⎥ 3.494 mm ⎢ ⎥ −1 UU = K11 (PK − K12 UK ) = ⎢ ⎥ ⎢ ⎥ 0 ⎢ ⎥ ⎢ ⎥ −3 ⎣−312.5 × 10 mm⎦ −1.138 × 10−3 ⎤ ⎡ ⎤ 30 × 106 N P7 ⎢ ⎥ ⎢ ⎥ PU = ⎣P8 ⎦ = ⎣−20 × 106 N⎦ P9 −20 × 106 N ⎡

The mid-span deﬂection is the displacement related to freedom 3) and is equal to 3.49 mm.

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element.

360 Stiffness method and ﬁnite-element modelling Element 1 The nodal displacements undergone by the end nodes of element 1 are collected in vector u(1) : ⎤

⎡

⎡ ⎤ u 0 mm L(1) ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢v ⎥ 0 mm ⎢ L(1) ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ v ⎥ ⎢ −3 ⎢ ⎥ 1.138 × 10 ⎥ ⎢ ⎥ u(1) = ⎢ L(1) ⎥ = ⎢ ⎢ ⎥ ⎥ ⎢ −3 mm⎥ ⎢uR(1) ⎥ ⎢ −156.2 × 10 ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢vR(1) ⎥ ⎣ 3.494 mm ⎦ ⎦ ⎣ vR(1)

0

The member actions are obtained from Eq. 9.11: p(1) = ku(1) + pF.m(1) T = 30 × 103 N −20 × 103 N 0 Nmm −30 × 103 N 0 N −50 × 106 Nmm The relevant constants of integration are then obtained from Eqs A.54: 1(1) = −124.3 × 10−12 mm−2 C 2(1) = −20.59 × 10−9 mm−1 C 3(1) = 1.138 × 10−3 C 4(1) = 0 mm C 5(1) = −8.368 × 10−6 C 6(1) = 0 mm C These can be substituted in Eqs 9.13 to determine the strain distribution along member 1. For example, the axial strain measured at the level of the ) at mid-span of the reference axis εr(1) (= u(1) ) and the curvature κ(1) (= −v(1) beam can be obtained by substituting z = 5000 mm in Eqs 9.13: εr(1) = u(1) (z = 5000) = −42.7 × 10−6 and κ(1) = −v(1) (z = 5000)

= 0.331 × 10−6 mm−1 which, as expected, corresponds to the same solution obtained in Example 5.1.

Stiffness method and ﬁnite-element modelling 361 The coefﬁcients deﬁning the expressions for the concrete internal axial force and moment are determined from Eqs A.57 and A.59: ac0(1) = −28.16 × 103 N ac1(1) = −6.701 Nmm−1 ac2(1) = 670.2 × 10−6 Nmm−2 bc0(1) = −66.96 × 103 Nmm bc1(1) = 15.65 × 103 N bc2(1) = −1.564 Nmm−1 Element 2 Similar to element 1, the terms describing the response of element 2 are calculated as: u(2) = uL(2) vL(2) vL(2) uR(2) vR(2) vR(2) = 156.2 × 10−3 3.494 0 − 312.5 × 10−3 0 − 1.138 × 10−3 p(2) = ku(2) + pF.m(2) T = 30 × 103 N 0 N 50 × 106 Nmm −30 × 103 N −20 × 103 N 0 Nmm 1(2) = 0 mm−2 C 2(2) = −331.3 × 10−9 mm−1 C 3(2) = 0 C 4(2) = 3.494 mm C 5(2) = −42.69 × 10−6 C 6(2) = −156.2 × 10−3 mm C The mid-span values of the strain variables (already calculated with element 1) could also have been determined with element 2 using the expressions of Eqs 9.13 at z = 0 mm.

9.4 Time analysis using AEMM When using the AEMM, deformations and stresses are calculated at two instants, immediately after loading at τ0 and after the effects of creep and shrinkage have taken place at τk . The instantaneous analysis at τ0 was presented in the previous section. The time analysis at time τk is outlined in the following. Creep and shrinkage effects are included in the stiffness analysis using equivalent nodal actions. As already discussed for the member loads, the set of equivalent nodal

362 Stiffness method and ﬁnite-element modelling actions to be used in the stiffness method correspond to the opposite of the reactions obtained when the supports of the element under consideration are assumed to be ﬁxed at both ends. The reactions produced by creep and shrinkage effects and by member loads are derived in Appendix A (Eqs A.66) and are reproduced below. ⎡

L2

⎤

ac2,0 ac1,0 L ⎢ ⎥ + + ac0,0 − Fe,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 a + a L L ⎢ ⎥ c1,0 c2,0 − Fe,0 − α3,k L − bc0,0 + bc2,0 ⎢ ⎥ ⎢ ⎥ 2 6 ⎥ pF.cr,k = ⎢ ⎢ ⎥ 2 ⎢ ⎥ a L L a c2,0 c1,0 ⎢ ⎥ Fe,0 + + ac0,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ −Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ 2 ac1,0 + ac2,0 L 5L ⎥ ⎣− ⎦ Fe,0 − α3,k L + bc0,0 + bc1,0 L + bc2,0 2 6 ⎤ ⎡ Ee,k Ac εsh,k ⎥ ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ ⎢− Ee,k Bc εsh,k ⎥ ⎥ pF.sh.k = ⎢ ⎥ ⎢ ⎢−Ee,k Ac εsh,k ⎥ ⎥ ⎢ ⎥ ⎢ 0 ⎦ ⎣ Ee,k Bc εsh,k ⎡ ⎤ ⎡ ⎤ 0 −L/2 ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ α3,k ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢Lα3,k /2⎥ pF.m,k = ⎢ ⎥p + ⎢ ⎥n ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ −L/2 ⎦ ⎣ −α3,k ⎦ L2 /12 Lα3,k /2

(9.15a)

(9.15b)

(9.15c)

where the constants α0,k , α1,k , α2,k , α3,k and α4,k are obtained from the cross-sectional rigidies at time τk using Eqs A.50a–e, respectively. The subscripts ‘m’, ‘cr’ and ‘sh’ used in pF.m,k , pF.cr,k and pF.sh,k indicate that the ﬁxed end reactions relate to either member loads, creep effects or shrinkage effects, respectively. The calculation at time τk of the cross-sectional rigidities RA,k , RB,k and RI,k required for input into Eqs A.50 has already been outlined in Chapter 5 for different types of cross-sections. The timedependent behaviour of concrete is represented by Ee,k and Fe,0 (given in Eqs 4.35 and 4.46), while εsh,k denotes the shrinkage strain. The coefﬁcients acj,0 and bcj,0 (with j = 0 to 2) that are necessary to deﬁne the expressions of the concrete internal actions are speciﬁed in Eqs A.57 and A.59.

Stiffness method and ﬁnite-element modelling 363 The time analysis can then be carried out by assembling the opposite of the vectors pF.m,k , pF.cr,k and pF.sh,k for each element into the loading vector of the structure, Pk , while using the cross-sectional properties calculated at τk in the determination of the stiffness coefﬁcients of Kk . When the unknown displacements and reactions are evaluated based on Eqs 9.9, the end actions of each element (i.e. member actions) can be obtained by combining the results of the stiffness analysis with those related to member loads, creep and shrinkage as follows: pk = kk uk + pF.m,k + pF.cr,k + pF.sh,k

(9.16)

The axial displacement uk and deﬂection vk can be calculated along the member axis using Eqs A.63 (repeated here for convenience): z3 2 1,k + α4,k n + β3,k z + C 6,k 5,k z + C uk = α2,k p + β2,k + α3,k C 6 2 3 2 z4 1,k z + C 2,k z + C 3,k z + C 4,k +C vk = α1,k p + β1,k 24 6 2

(9.17a) (9.17b)

where the constants αj,k (with j = 0 to 4) and βj,k (with j = 1 to 3) are given in 6,k are 1,k to C Eqs A.50 and A.64, respectively and the constants of integration C given in Eqs A.67. The strain diagram at any point along an element can be obtained by differentiating Eqs 9.17 to give: z2 1,k + α4,k n + β3,k z + C 5,k + α3,k C uk = α2,k p + β2,k 2 z2 1,k z + C 2,k +C vk = α1,k p + β1,k 2

(9.18a) (9.18b)

from which the stresses may be evaluated following the procedures illustrated in Chapter 5.

Example 9.2 The deﬂection at time τk and the variables deﬁning the strain diagram (εr,k and κk ) at mid-span of the simply-supported beam analysed in Example 9.1 are to be determined, as well as the actions resisted by the two elements. The applied loads are assumed to remain constant with time. The cross-sectional and material properties of the beam are those of the reinforced concrete section considered in Example 5.3. The analysis is to be carried out using the stiffness method assuming the same two elements and freedom numbering as adopted in Example 9.1. All units are in mm and N, unless noted otherwise. From Example 5.3: Ee,k = 9524 MPa Fe,0 = −0.333 ϕ(τk , τ0 ) = 2.5

364 Stiffness method and ﬁnite-element modelling χ (τk , τ0 ) = 0.65 εsh (τk ) = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4 RA,k = 2175 × 106 N RB,k = 273.7 × 109 Nmm RI,k = 113.2 × 1012 Nmm2 and from Example 5.1: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 As for Example 9.1: T UU,k = U1,k U2,k U3,k U4,k U5,k U6,k T T UK,k = U7,k U8,k U9,k = 0 0 0 T PU,k = P7,k P8,k P9,k From Eqs A.50: α0,k = 171.4 × 1021 N2 mm2 α1,k = 12.69 × 10−15 N−1 mm−2 α2,k = 1597 × 10−15 N−1 mm−1 α3,k = 125.8 mm α4,k = −459.7 × 10−12 N−1 The stiffness matrix for both elements 1 and 2 are identical and calculated at time τk as (Eq. 9.2a): ⎡ ⎤ 435.0 × 103 0 −54.74 × 106 −435.0 × 103 0 −54.74 × 106 ⎢ ⎥ 7.563 × 103 18.91 × 106 0 −7.563 × 103 18.91 × 106 ⎥ ⎢ ⎢ ⎥ 9 6 6 9 ⎢ 54.74 × 10 −18.91 × 10 24.62 × 10 ⎥ 69.92 × 10 ⎥ ke = ⎢ ⎢ ⎥ 435.0 × 103 0 −54.74 × 106 ⎥ ⎢ ⎢ ⎥ 3 6 ⎣ sym 7.563 × 10 −18.91 × 10 ⎦ 69.92 × 109

Stiffness method and ﬁnite-element modelling 365 The set of reactions required to account for the member load p = 4 N/mm and for shrinkage are (Eqs 9.15b and c): ⎡

⎤ 0

⎡

⎤ 0N

⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢−8.3 × 106 Nmm⎥ pF.m,k(1) = pF.m,k(2) = ⎢ ⎥p = ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ −10 × 103 N ⎥ ⎣ ⎦ ⎣ ⎦ L2 /12 8.3 × 106 Nmm ⎤ ⎡ ⎤ ⎡ ⎡ ⎤ 6 N E A ε −1014 × 10 a c sh,k e,k sh,k ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ 0 ⎥ ⎢ ⎥ 0 0N ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ 6 ⎢−bsh,k ⎥ ⎢−Ee,k Bc εsh,k ⎥ ⎢ 99.78 × 10 Nmm ⎥ pF.sh,k(1) = pF.sh,k(2) = ⎢ ⎥=⎢ ⎥=⎢ ⎥ ⎥ ⎢ ⎢−a ⎥ ⎢− ⎥ 6 ⎢ sh,k ⎥ ⎢ Ee,k Ac εsh,k ⎥ ⎢ 1014 × 10 N ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ 0 ⎥ ⎢ ⎥ 0 N 0 ⎦ ⎣ ⎦ ⎣ ⎣ ⎦ −99.78 × 106 Nmm bsh,k Ee,k Bc εsh,k The vectors pF.cr,k(1) and pF.cr,k(2) need to be evaluated for the two elements separately. From Example 9.1: ac0(1),0 = −28.16 × 103 N ac1(1),0 = −6.701 Nmm−1 ac2(1),0 = 670.2 × 10−6 Nmm−2 bc0(1),0 = −66.96 × 103 Nmm bc1(1),0 = 15.65 × 103 N bc2(1),0 = −1.564 Nmm−1 ac0(2),0 = −44.91 × 103 N ac1(2),0 = 2.788 × 10−12 Nmm−1 ac2(2),0 = 670.2 × 10−6 Nmm−2 bc0(2),0 = 39.05 × 106 Nmm bc1(2),0 = −6.509 × 10−12 N bc2(2),0 = −1.564 Nmm−1

366 Stiffness method and ﬁnite-element modelling From Eq. 9.15a: ⎡

⎡ ⎤ ⎤ −13.11 × 103 N −13.11 × 103 N ⎢ ⎢ ⎥ ⎥ ⎢ 2.748 × 103 N ⎥ ⎢ −2.748 × 103 N ⎥ ⎢ ⎢ ⎥ ⎥ 6 ⎢−1.799 × 106 Nmm⎥ ⎢ ⎥ ⎥ and pF.cr(2),k = ⎢−15.54 × 10 Nmm⎥ pF.cr(1),k = ⎢ ⎢ 13.11 × 103 N ⎥ ⎢ 13.11 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎣ −2.748 × 103 N ⎦ ⎣ 2.748 × 103 N ⎦ 15.54 × 106 Nmm 1.799 × 106 Nmm

After assembly, the sub-matrices of Kk and the loading vector Pk of the whole structure at τk are: ⎤ ⎡ 69.92 × 109 54.74 × 106 −18.91 × 106

⎢ ⎢ ⎢ ⎢ K11,k = ⎢ ⎢ ⎢ ⎢ ⎣ ⎡

870.1 × 103

⎢ K22,k = ⎢ ⎣

0

−109.5 × 106 −435.0 × 103

0 15.13 × 103

0

0

139.8 × 109

54.74 × 106 435.0 × 103

sym

−54.74 × 106

⎢ ⎢−435.0 × 103 ⎢ ⎢ ⎢ 0 K12,k = ⎢ ⎢ ⎢ 54.74 × 106 ⎢ ⎢ 0 ⎣ ⎡

24.63 × 109

0 435.0 × 103 sym

⎤

18.91 × 106

0

0

0

0

⎥ ⎥ 18.91 × 106 ⎥ ⎥ ⎥ 24.63 × 109 ⎥ ⎥ −54.74 × 106⎦ 54.74 × 106 ⎥

69.92 × 109

⎥ ⎥ ⎥ ⎥ 3 3 −7.56 × 10 −7.56 × 10 ⎥ ⎥ ⎥ 6 6 18.91 × 10 −18.91 × 10 ⎥ ⎥ ⎥ 0 0 ⎦ 6 0 −18.91 × 10 ⎤ 0 0 ⎥ ⎥ 7.563 × 103 0 ⎦ 7.563 × 103

T K21,k = K12,k

Pk = [89.66 × 106 0

25.50 × 103

0

−1057 × 103

89.66 × 106

(P7 + 1027 × 103 ) (P8 + 7.252 × 103 ) (P7 + 7.252 × 103 )]T

From Eqs 9.9, unknown displacements UU,k and reactions PU,k are obtained: ⎤ ⎡ 4.781 × 10−3 ⎥ ⎢ ⎢ −3.033 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ 13.65 mm ⎥ −1 UU,k = K11,k PK,k − K12,k UK,k = ⎢ ⎥ and ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ −6.066 mm ⎦ ⎣ −4.780 × 10−3

Stiffness method and ﬁnite-element modelling 367 ⎤ 30 × 106 N P7,k ⎥ ⎢ ⎢ ⎥ PU,k = ⎣P8,k ⎦ = ⎣−20 × 106 N⎦ ⎤

⎡

P9,k

⎡

−20 × 106 N

The mid-span deﬂection at τk (associated with freedom 3) is 13.65 mm which has increased from its initial value of 3.49 mm.

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element. Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: ⎤ ⎡ ⎡ ⎤ uL(1),k 0 mm ⎥ ⎢ ⎢ ⎥ ⎢ vL(1),k ⎥ ⎢ ⎥ 0 mm ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ v ⎥ −3 ⎢ L(1),k ⎥ ⎢4.781 × 10 ⎥ u(1),k = ⎢ ⎥=⎢ ⎥ ⎢uR(1),k ⎥ ⎢ −3.033 mm ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎣vR(1),k ⎦ ⎣ 13.65 mm ⎦ 0 vR(1),k p(1),k = kk u(1),k + pF.m(1),k + pF.cr(1),k + pF.sh(1),k T = 30 × 103 −20 × 103 0 −30 × 103 0 −50 × 106 As expected, the member actions are identical to the instantaneous values as the structure is statically determinate. From Eqs A.67: 1(1),k = −323.6 × 10−12 mm−2 C 2(1),k = −416.7 × 10−9 mm−1 C 3(1),k = 4.780 × 10−3 C 4(1),k = 0 mm C 5(1),k = −539.6 × 10−6 C 6(1),k = 0 mm C The axial strain measured at the level of the reference axis and the curvature at mid-span are determined by substituting the calculated constants of integration into Eqs 9.18 with z = 5000 mm: i.e. εr(1),k = u(1),k = −641.4 × 10−6 and κ(1),k =

= 1.225 × 10−6 mm−1 . As expected, these results are identical to those −v(1),k calculated in Example 5.3.

368 Stiffness method and ﬁnite-element modelling Element 2 The nodal displacements and the member actions associated with the end nodes of element 1 are: ⎤ −3.033 mm ⎥ ⎢ ⎥ ⎢ ⎢ vL(2),k ⎥ ⎢ 13.65 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ v 0 ⎥ ⎢ L(2),k ⎥ ⎢ u(2),k = ⎢ ⎥=⎢ ⎥ ⎢uR(2),k ⎥ ⎢ −6.066 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 ⎦ ⎣vR(2),k ⎦ ⎣ −3 −4.780 × 10 vR(2),k ⎡

uL(2),k

⎤

⎡

p(2),k = kk u(1),k + pF.m(1),k + pF.cr(1),k + pF.sh(1),k = 30 × 103 0 50 × 106 −30 × 103 −20 × 103

T 0

9.5 Time analysis using SSM When using the SSM, the time domain is discretised into a number of time instants τi (with i = 1, . . . , k) as shown in Fig. 4.3. As for the AEMM discussed in the previous section, the time-dependent behaviour of the concrete is included in the analysis using equivalent nodal actions that correspond to the opposite of the reactions obtained when the ends of the element are ﬁxed and the member is loaded and subject to creep and shrinkage. These reactions are determined at a particular instant in time, here referred to as τk , and are expressed as the vectors pF.m,k , pF.cr,k and pF.sh,k in Eqs A.91. Most of the notation used in the expressions for pF.m,k , pF.cr,k and pF.sh,k has already been deﬁned in the previous section. The procedure for the SSM and the various constants and coefﬁcients are derived in the Section A.5.3 and presented in Eqs A.71– A.91. The loading vector Pk is assembled, including the contributions of pF.m,k , pF.cr,k and pF.sh,k for every element, and the stiffness coefﬁcients for Kk are calculated based on the cross-sectional rigidities determined at time τk . The solution at time τk is obtained using Eqs 9.9. Post-processing to obtain stresses and strains on particular cross-sections is as described previously. The element end actions are evaluated from Eq. 9.16 and the axial displacement and deﬂection at any distance z along the element are expressed by Eqs A.77. The variables describing the strain diagram at time τk (εr,k = uk and κk = −vk ) are obtained from Eqs A.80.

Example 9.3 The simply-supported beam analysed in Example 9.2 is to be re-analysed using the stiffness method and using the SSM to handle the time effects. The time domain is discretised into three time instants: τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. The deﬂection and the axial strain at the level of the

Stiffness method and ﬁnite-element modelling 369 reference axis and curvature at mid-span are to be calculated at each of these time instants. In addition, the member actions at each time step are determined for both elements. As in Examples 9.1 and 9.2, two elements are considered with freedom numbering as shown in Fig. 9.5. The cross-section of the beam at mid-span was previously analysed using the SSM in Example 5.5, where: Ec,0 = 25 GPa Ec,1 = 28 GPa Ec,2 = 30 GPa Fe,1,0 = −1.8 Fe,2,0 = −0.986 Fe,2,1 = −2.214 εsh (τ0 ) = εsh,0 = 0 εsh (τ1 ) = εsh,1 = −300 × 10−6 εsh (τ2 ) = εsh,2 = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4 Similarly to Example 9.1, the sets of known and unknown displacements and unknown actions for the three time steps τj (with j = 1, 2, 3) are: T UU,j = U1,j U2,j U3,j U4,j U5,j U6,j T T UK,j = U7,j U8,j U9,j = 0 0 0 T PU,j = P7,j P8,j P9,j From Examples 5.1 and 5.5: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 RA,1 = 5456 × 106 N RB,1 = 596.4 × 109 Nmm RI,1 = 241.9 × 1012 Nmm2 RA,2 = 5811 × 106 N RB,2 = 631.3 × 109 Nmm RI,2 = 255.8 × 1012 Nmm2

370 Stiffness method and ﬁnite-element modelling From Eqs A.50: α0,1 = 792.3 × 1021 N2 mm2 α1,1 = 6.214 × 10−15 N−1 mm−2 α2,1 = 686.6 × 10−15 N−1 mm−1 α3,1 = 110.5 mm α4,1 = −203.1 × 10−12 N−1 α0,2 = 964.4 × 1021 N2 mm2 α1,2 = 5.658 × 10−15 N−1 mm−2 α2,2 = 618.4 × 10−15 N−1 mm−1 α3,2 = 109.3 mm α4,2 = −193.3 × 10−12 N−1

Short-term analysis (τ0 = 28 days) The solution at time τ0 is identical to that presented in Example 9.1.

Time analysis – SSM (τ1 = 100 days) The stiffness matrix for elements 1 and 2 is determined using Eq. 9.2a with the rigidities calculated at time τ1 : ⎡ ⎤ 1091 × 103 0 −119.3 × 106 −1091 × 103 0 119.3 × 106 ⎢ ⎥ ⎢ 16.97 × 103 42.42 × 106 0 −16.97 × 103 42.42 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ 9 6 6 9 ⎥ ⎢ 154.4 × 10 119.3 × 10 −42.42 × 10 57.66 × 10 ⎥ k1 = ⎢ ⎢ ⎥ ⎢ 1091 × 103 0 −119.3 × 106 ⎥ ⎢ ⎥ ⎢ sym 16.97 × 103 −42.42 × 106 ⎥ ⎣ ⎦ 154.4 × 109

Since, the external loads are constant in time, the sets of reactions required to account for the member load p = 4 N/mm (i.e. pF,m(1),1 and pF,m(2),1 ) are identical to those determined in Example 9.1 at τ0 . Shrinkage is accounted for using Eq. A.91b with ⎤ ⎡ ⎤ −1491 × 106 Ec,1 Ac εsh,1 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 6 ⎢−Ec,1 Bc εsh,1 ⎥ ⎢ 146.7 × 10 ⎥ pF.sh(1),1 = pF.sh(2),1 = ⎢ ⎥=⎢ ⎥ ⎢−Ec,1 Ac εsh,1 ⎥ ⎢ 1491 × 106 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎦ ⎣ ⎦ ⎣ ⎡

Ec,1 Bc εsh,1

−146.7 × 106

Stiffness method and ﬁnite-element modelling 371 From Example 9.1, for element 1: ac0(1),0 = −28.16 × 103 Nmm2 ac1(1),0 = −6.701 Nmm−1 ac2(1),0 = 670.2 × 10−6 Nmm−2 bc0(1),0 = −66.96 × 103 Nmm bc1(1),0 = 15.65 × 103 N bc2(1),0 = −1.564 Nmm−1 and for element 2: ac0(2),0 = −44.91 × 103 Nmm2 ac1(2),0 = 2.788 × 10−12 Nmm−1 ac2(2),0 = 670.2 × 10−6 Nmm−2 bc0(2),0 = 39.05 × 106 Nmm bc1(2),0 = −6.509 × 10−12 N bc2(2),0 = −1.564 Nmm−1 From Eq. A.91, the creep effects are included in pF,cr(1),1 and pF,cr(2),1 : ⎤ ⎤ ⎡ −70.8 × 103 −70.8 × 103 ⎥ ⎥ ⎢ ⎢ ⎢ 14.74 × 103 ⎥ ⎢−14.74 × 103 ⎥ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎢−9.968 × 106 ⎥ ⎢−83.67 × 106 ⎥ pF.cr(1),1 = ⎢ and pF.cr(2),1 = ⎢ ⎥ ⎥ ⎢ 70.8 × 103 ⎥ ⎢ 70.8 × 103 ⎥ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎣−14.74 × 103 ⎦ ⎣ 14.74 × 103 ⎦ 83.67 × 106 9.968 × 106 ⎡

After assembly, the sub-matrices of K1 and the load vector P1 of the whole structure at τ1 are: ⎤

⎡ 154.4 × 109 119.3 × 106 −42.42 × 106

⎢ ⎢ ⎢ ⎢ K11,1 = ⎢ ⎢ ⎢ ⎢ ⎣

2182 × 103

0 119.3 × 103

sym

57.66 × 109

0

−238.5 × 106 −1091 × 103 0

0

308.9 × 109

119.3 × 106 1091 × 103

0

⎥ ⎥ 42.42 × 106⎥ ⎥ ⎥ 57.66 × 109⎥ ⎥ −119.3 × 106⎦ 119.3 × 106⎥

154.4 × 109

372 Stiffness method and ﬁnite-element modelling ⎡ 0 −119.3 × 106 42.42 × 106 ⎢ ⎢ −1091 × 103 0 0 ⎢ ⎢ 3 ⎢ 0 −16.97 × 10 −16.97 × 103 K12,1 = ⎢ ⎢ ⎢ 119.3 × 106 42.42 × 106 −42.42 × 106 ⎢ ⎢ 0 0 0 ⎣ 0 0 −42.42 × 106 ⎡ ⎤ 0 0 1091 × 103 ⎢ ⎥ K22,1 = ⎣ ⎦ 16.97 × 103 0

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦

16.97 × 103

sym T K21,1 = K12,1

P1 = − 128.4 × 106 0

49.48 × 103 0 −1592 × 103 128.4 × 106 T (P7 + 1562 × 103 ) (P8 − 4.742 × 103 ) (P7 − 4.742 × 103 )

Solving for the unknown displacements and reactions using Eqs 9.9 gives: ⎤ ⎡ 3.042 × 10−3 ⎥ ⎢ ⎥ ⎢ −1.792 ⎥ ⎢ ⎥ ⎢ ⎢ 9.063 ⎥ −1 UU,1 = K11,1 PK,1 − K12,1 UK,1 = ⎢ ⎥ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ −3.583 ⎦ ⎣ −3 −3.042 × 10 ⎤ ⎡ ⎤ ⎡ 30 × 106 P7,1 ⎥ ⎢ ⎥ ⎢ PU,1 = ⎣P8,1 ⎦ = ⎣−20 × 106 ⎦ P9,1

−20 × 106

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element. Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: T u(1),1 = 0 0 3.042 × 10−3 −1.792 9.063 0 p(1),1 = k1 u(1),1 + pF.m(1),1 + pF.cr(1),1 + pF.sh(1),1 T = 30 × 103 −20 × 103 0 −30 × 103 0 −50 × 106

Stiffness method and ﬁnite-element modelling 373 Using Eqs A.90: β1(1),1 = 33.36 × 10−15 mm β2(1),1 = 4.088 × 10−12 mm2 β3(1),1 = −2.211 × 10−9 mm−1 From Eqs A.79: 1(1),1 = −280 × 10−12 mm−2 C 2(1),1 = −141.7 × 10−9 mm−1 C 3(1),1 = 3.042 × 10−3 C 4(1),1 = 0 mm C 5(1),1 = −303.7 × 10−6 C 6(1),1 = 0 mm C The axial strain and curvature are calculated at mid-span by substituting z = 5000 mm into Eqs A.68 giving εr(1),1 = u(1),1 = −385.7 × 10−6 and κ(1),1 = = 0.841 × 10−6 mm−1 , which are the same as the results of Example 5.5 −v(1),1 at τ1 . From Eqs A.82 and A.84: ac0(1),1 = 101.7 × 103 Nmm2 ac1(1),1 = −14.19 Nmm−1 ac2(1),1 = 1419 × 10−6 Nmm−2 bc0(1),1 = 25.97 × 106 Nmm bc1(1),1 = 10.39 × 103 N bc2(1),1 = −1.039 Nmm−1 Element 2 T u(2),1 = −1.792 9.063 0 −3.583 0 −3.042 × 10−3 T p(2),1 = 30 × 103 0 50 × 106 −30 × 103 −20 × 103 0

374 Stiffness method and ﬁnite-element modelling

Time analysis – SSM (τ2 = 30,000 days) Following the procedure outlined for the time analysis at τ1 , the stiffness matrix for elements 1 and 2 is based on the rigidities at τ2 : ⎡ ⎤ 1162 × 103 0 −126.3 × 106 −1162 × 103 0 126.3 × 106 ⎢ ⎥ ⎢ ⎥ 17.97 × 103 44.95 × 106 0 −17.98 × 103 44.95 × 106 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ 163.5 × 109 126.3 × 106 −44.95 × 106 61.19 × 109 ⎥ k2 = ⎢ ⎢ ⎥ ⎢ 1162 × 103 0 −126.3 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ sym 19.97 × 103 −44.95 × 106 ⎥ ⎣ ⎦ 163.5 × 109

The equivalent nodal loads to account for shrinkage and creep in each element are: ⎤ ⎡ ⎤ ⎡ −3196 × 106 Ec,2 Ac εsh,2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 6 ⎢−Ec,2 Bc εsh,2 ⎥ ⎢ 314.3 × 10 ⎥ pF.sh(1),2 = pF.sh(2),2 = ⎢ ⎥=⎢ ⎥ ⎢−Ec,2 Ac εsh,2 ⎥ ⎢ 3196 × 106 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎦ ⎣ ⎦ ⎣ 6 Ec,2 Bc εsh,2 −314.3 × 10 ⎤ ⎡ 134.2 × 103 ⎥ ⎢ ⎢ 21.29 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢−68.29 × 106 ⎥ pF.cr(1),2 = ⎢ ⎥ ⎢−134.2 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎣−21.29 × 103 ⎦ 174.7 × 106 ⎤ ⎡ 134.2 × 103 ⎥ ⎢ ⎢−21.29 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢−174.7 × 106 ⎥ pF.cr(2),2 = ⎢ ⎥ ⎢−134.2 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎣ 21.29 × 103 ⎦ 68.3 × 106 Assembling of the stiffness matrix K2 and load vector P2 for the whole structure: ⎡

162.5 × 109 126.3 × 106 −44.95 × 106

⎢ ⎢ ⎢ ⎢ K11,2 = ⎢ ⎢ ⎢ ⎣

2324 × 103

0 35.96 × 103

sym

61.19 × 109

⎤ 0

−252.5 × 106 −1162 × 103 0

0

327.1 × 109

126.3 × 106 1162 × 103

0

⎥ ⎥ ⎥ 44.95 × 106 ⎥ ⎥ 61.19 × 109 ⎥ ⎥ −126.3 × 106 ⎦ 126.3 × 106

163.5 × 109

⎡

−126.3 × 106 ⎢ ⎢ −1162 × 103 ⎢ ⎢ ⎢ 0 K12,2 = ⎢ ⎢ ⎢ 126.3 × 106 ⎢ ⎢ 0 ⎣ 0 ⎡ ⎢ K22,2 = ⎢ ⎣

Stiffness method and ﬁnite-element modelling 375 ⎤ 44.95 × 106 0 ⎥ ⎥ 0 0 ⎥ ⎥ −17.98 × 103 −17.98 × 103 ⎥ ⎥ ⎥ 44.95 × 106 −44.95 × 106 ⎥ ⎥ ⎥ 0 0 ⎦ 0 −44.95 × 106 ⎤

1162 × 103

0

0

17.98 × 103

0

⎥ ⎥ ⎦

17.98 × 103

sym T K21,2 = K12,2

P2 = − 237.7 × 106

0

62.57 × 103

−3092 × 103

0

(P7 + 3062 × 103 )

(P8 − 11.29 × 103 )

237.7 × 106

T (P7 − 11.29 × 103 )

Solving for the unknown displacements and reactions using Eqs 9.9 gives: ⎡ ⎢ ⎢ ⎢ ⎢ ⎢ −1 UU,2 = K11,2 PK,2 − K12,2 UK,2 = ⎢ ⎢ ⎢ ⎢ ⎢ ⎣

4.71 × 10−3 −3.172 13.51 0 −6.344 −4.71 × 10−3

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ and ⎥ ⎥ ⎥ ⎥ ⎦

⎤ ⎤ ⎡ 30 × 106 P7,2 ⎥ ⎥ ⎢ ⎢ 6⎥ PU,2 = ⎣P8,2 ⎦ = ⎢ ⎣−20 × 10 ⎦ ⎡

−20 × 106

P9,2

Post-processing: Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: u(1),2 = 0

0

4.71 × 10−3

p(1),2 = 30 × 103

−20 × 103

−3.172

13.51

0 −30 × 103

T 0 0 −50 × 106

T

376 Stiffness method and ﬁnite-element modelling and with: β1(1),2 = 45.46 × 10−15 mm β2(1),2 = 6.247 × 10−12 mm2 β3(1),2 = −6.542 × 10−9 mm−1 1(1),2 = −334.1 × 10−12 mm−2 C 2(1),2 = −385.1 × 10−9 mm−1 C 3(1),2 = 4.71 × 10−3 C 4(1),2 = 0 mm C 5(1),2 = −563.0 × 10−6 C 6(1),2 = 0 mm C The axial strain and curvature calculated at mid-span (i.e. at z = 5000 mm) at τ2 are: εr(1),2 = u(1),2 = −385.7 × 10−6 and κ(1),2 = −v(1),2 = 0.841 × 10−6 mm−1

Element 2 T u(2),2 = −3.172 13.51 0 −6.344 0 −4.71 × 10−3 T p(2),2 = 30 × 103 0 50 × 106 −30 × 103 −20 × 103 0

9.6 Time analysis using the ﬁnite-element method The ﬁnite-element method is a well-established method of analysis extensively used in all disciplines of engineering and its use is well reported in the literature (Ref. 2). Only the main aspects related to this method are outlined here, with particular attention placed on how time effects can be included in the analysis. For illustrative purposes, a displacement-based line element similar to the one described for the stiffness method is considered in the following. Its detailed formulation is outlined in Appendix A. The proposed approach for the inclusion of time effects in ﬁnite-element analysis can be extended to any other type of ﬁnite element, i.e. displacement-based, force-based or mixed elements. For ease of notation, subscripts deﬁning particular time instants are included only when the instant considered is not clear from the context. The weak form of the problem used to derive the proposed line ﬁnite element is obtained by means of the principle of virtual work as outlined in Section A.3. Restating Eq. A.18: ri · A eˆ dz = q · eˆ dz (9.19) L

L

Stiffness method and ﬁnite-element modelling 377 in which q contains the external distributed loads n and p (Fig. 9.3) and the vector e contains the independent variables deﬁning the displacement ﬁeld for the Euler– Bernoulli beam model consisting of the axial displacement measured at the level of the reference axis u and the deﬂection v. That is: n q= (9.20a) p u e= (9.20b) v The variables deﬁning the strain diagram, i.e. εr and κ, are obtained by differentiating e as follows (Eq. A.16): εr u ε= = = Ae (9.21) κ −v where the differential operator A is expressed (with ∂ ≡

∂ 0 A= 0 −∂ 2

d (·) ) by: dz

and the expression for the axial strain at a point in the member ε is: ε = εr + yκ = u − yv = 1 y ε

(9.22)

(9.23)

The internal resultants collected in ri (i.e. the internal axial force and moment) have been deﬁned in Chapter 5 for different types of cross-sections and may be expressed as (Eqs A.11): ri = Dε + fcr − fsh

(9.24)

where the terms related to creep and shrinkage vanish when performing an instantaneous analysis. The vectors and matrices in Eq. 9.24 are expanded in Eqs A.13 (and were used in Chapters 5 and 7). The vectors f cr and f sh depicting the creep and shrinkage response have been expressed in terms of their components fcrN , fcrM , fshN , and fshM to simplify the notation and, for the AEMM, are given by Eqs A.14 and, for the SSM, are given in Eqs A.15. The proposed ﬁnite-element formulation relies on the approximation of the independent variables deﬁning the kinematic response, i.e. u and v previously collected in e (Eq. 9.20b), as follows: e ≈ N e de

(9.25)

where de are the nodal displacements of the ﬁnite element under consideration and Ne contains the shape functions that describe the variations of these displacements along the element length.

378 Stiffness method and ﬁnite-element modelling Similarly to the stiffness relationship of Eq. 9.1, the governing system of equations describing the behaviour of a line element can be expressed in terms of nodal displacements de and actions pe : pe = ke de

(9.26)

where ke is the ﬁnite element stiffness matrix (given in Eq. A.25a and reproduced here as Eq. 9.27) and pe is the load vector accounting for the contributions of pe.m , pe.cr , and pe.sh (given in Eqs A.25b and A.26): ke =

T

L

(A Ne ) D ε dz =

L

(A Ne )T D (A Ne ) dz

(9.27)

The derivation for a particular ﬁnite element is carried out here for the 7 DOF element depicted in Fig. 9.6. In this case the axial and vertical displacements are approximated by parabolic and cubic polynomials, respectively. The nodal displacements and shape functions expressing this approximation are outlined in Eqs A.27–A.30 and the stiffness matrix and load vector related to member loads n and p are given in Eqs A.31 and A.32 (reproduced below): ⎡ −4RB −3RB −8RA RA ⎢ 7RA ⎢ 3L 2 L 3L 3L L ⎢ ⎢ ⎢ −4RB 12RI 6RI 8RB −4RB ⎢ ⎢ L2 L3 L2 L2 L2 ⎢ ⎢ ⎢ −3RB 6RI 4RI 4RB −RB ⎢ ⎢ 2 L L L L ⎢ L ⎢ ⎢ −8R 4RB 8RB 16RA −8RA ke = ⎢ A ⎢ 2 ⎢ 3L L 3L 3L L ⎢ ⎢ R −4RB −RB −8RA 7RA ⎢ A ⎢ 2 ⎢ 3L L 3L 3L L ⎢ ⎢ −12RI −6RI −8RB 4RB ⎢ 4RB ⎢ 3 2 2 ⎢ L2 L L L L2 ⎢ ⎣ −RB 6RI 2RI 4RB −3RB L L L L L2

T L L L2 2L L L L2 pe.m = n p p n n p − p 6 2 12 3 6 2 12 qR uM

uL

qL vL

4RB L2 −12RI L3 −6RI L2 −8RB L2 4RB L2 12RI L3 −6RI L2

⎤ −RB ⎥ L ⎥ ⎥ ⎥ 6RI ⎥ ⎥ L2 ⎥ ⎥ ⎥ 2RI ⎥ ⎥ ⎥ L ⎥ ⎥ 4RB ⎥ ⎥ (9.28) ⎥ L ⎥ ⎥ −3RB ⎥ ⎥ ⎥ L ⎥ ⎥ ⎥ −6RI ⎥ ⎥ L2 ⎥ ⎥ ⎦ 4RI L

uR

vR

z L

Figure 9.6 Nodal displacements of the 7 DOF ﬁnite element.

(9.29)

Stiffness method and ﬁnite-element modelling 379 For illustrative purposes and to better outline all the steps involved in the solution process, the integrals in the expressions for ke (Eq. 9.27) and pe.m (Eq. A.26a) have been solved analytically throughout this chapter and in Appendix A. However, numerical integration could be easily implemented if preferred. Even if not carried out in the following, static condensation could be used to handle the internal freedom (Ref. 2). The stiffness relationship of Eq. 9.26 is expressed in the local coordinates of the member (assuming the z-axis coincides with the member axis). This relationship must be transformed and expressed in global coordinates (i.e. coordinate system applicable to the whole structure) following the procedure previously outlined for the stiffness method in Eqs 9.3–9.6. The transformation matrix T for the 7 DOF ﬁnite element is: ⎡

c

s

⎢ ⎢−s c ⎢ ⎢ ⎢0 0 ⎢ T=⎢ ⎢0 0 ⎢ ⎢0 0 ⎢ ⎢ ⎣0 0 0

0 0

0

0 0

0

1 0

0

0 1

0

0

0

c

0

0 −s

0 0 0

0

⎤ 0 0 ⎥ 0 0⎥ ⎥ ⎥ 0 0⎥ ⎥ 0 0⎥ ⎥ ⎥ s 0⎥ ⎥ ⎥ c 0⎦

(9.30)

0 1

The assembly procedure required to yield the stiffness relationship applicable to the whole structure is similar to the one utilised for the stiffness method. This produces relationships similar to those already presented in Eqs 9.7 and 9.8. The unknown displacements and reactions can be solved using Eqs 9.9. When the analysis is completed, the solution is post-processed and, for each element, the different variables describing its structural response are determined. For example, the variables deﬁning the strain diagram can be obtained by substituting the approximated displacements (Eq. 9.25) into Eq. 9.21 (Eqs A.34):

3 4 1 4 8 4 u = − uL + uM − uR + z (9.31a) u − u + u L M R L L L L2 L2 L2

6 4 6 2 12 6 12 6 v = − 2 v L − θL + 2 v R − θR + vL + 2 θL − 3 vR + 2 θR z (9.31b) L L L L L3 L L L where all nodal displacements are deﬁned in Fig. 9.6. Considering the post-processing of the instantaneous analysis, the stress resultants resisted by the concrete component can be expressed as (Eqs A.35a and d): Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0 = ac0,0 + ac1,0 z

(9.32a)

Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0

(9.32b)

= bc0,0 + bc1,0 z

where the adopted subscript ‘0’ has been introduced to highlight that these expressions are only applicable at time τ0 . The coefﬁcients ac0,0 , ac1,0 , bc0,0 and bc1,0 are given in Eqs A.35.

380 Stiffness method and ﬁnite-element modelling As previously mentioned, for the calculation of the terms in ke and pe.m (Eqs 9.28 and 9.29) numerical integration could be used. For example, the axial force and moment resisted by the concrete at τ0 could be calculated by numerical integration of the expressions presented in Eqs A.33. For clarity, an approach similar to the one already presented for the stiffness method has been adopted in which the variables are represented using polynomials that, in this case, are linear for both Nc,0 and Mc,0 (Eqs 9.32). Obviously, numerical integration could be easily implemented if preferred in the proposed solution process. The use of the linear polynomial has been determined by considering the degree of the polynomials adopted to approximate the displacements u and v in Eqs A.27–A.29. Based on these the variations of both u and v deﬁning the strain diagram (Eq. 9.31) are linear functions of z and, as a consequence, so to are the expressions for Nc,0 and Mc,0 in Eqs 9.32. 9.6.1 Load vector to account for time effects using the AEMM The calculation of the loading vector describing creep effects, i.e. pe.cr introduced in Eq. A.26b, requires the knowledge of the axial force fcrN and moment fcrM included in f cr which, when considering the AEMM, is deﬁned in Eqs A.14a and c. Both fcrN and fcrM are found by multiplying the axial force and moment resisted by the concrete at time τ0 by the material coefﬁcient Fe,0 : fcrN = Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z

(9.33a) (9.33b)

Equations 9.33 highlight that it is necessary to record the stress state of the concrete obtained from the instantaneous analysis before initiating the time analysis. When using numerical integration for the calculation of the stress resultants in the concrete, the values of the concrete axial force and moment at particular locations at time τ0 along each member are stored. These locations are usually those required by the numerical integration of Eqs A.25 and A.27. Another option, used in the following (and in Appendix A), is to identify polynomials capable of describing the variations of the concrete axial force and moment along each element and to store the relevant coefﬁcients. This has already been carried out in Eqs 9.32. The loading vector describing shrinkage effects pe.sh is expressed as Eq. A.26c. If it assumed that the shrinkage of a member does not vary along its length, the axial force fshN and moment fshM required to deﬁne f sh in Eq. A.26c are given by: fshN =

Ac

fshM =

Ac

Ee,k εsh,k dA = Ee,k Ac εsh,k

(9.34a)

y Ee,k εsh,k dA = Ee,k Bc εsh,k

(9.34b)

Based on the expressions for fcrN and fcrM (Eqs 9.33) and fshN and fshM (Eqs 9.34) and the deﬁnitions of pe.cr and pe.sh (Eqs A.26b and c), it is possible to determine the load vectors which account for creep and shrinkage. These are derived in Appendix A and given in Eqs A.36 and A.37.

Stiffness method and ﬁnite-element modelling 381 9.6.2 Load vector to account for time effects using the SSM Assuming the time-dependent behaviour of the concrete to be modelled by means of the SSM the expressions for fcrN and fcrM to be included in f cr are (Eqs A.15): fcrN =

fcrM =

k−1 i=0 Ac k−1 i=0 Ac

Fe,k,i σc,i dA =

k−1

Fe,k,i Nc,i

(9.35a)

i=0

yFe,k,i σc,i dA =

k−1

Fe,k,i Mc,i

(9.35b)

i=0

where the variation of the concrete stress resultants has also been described by a linear polynomial. For any time τi , the axial force and moment resisted by the concrete is calculated using the linear polynomials as given in Eqs A.41. Substituting the polynomial describing the variations of Nc,i and Mc,i expressed in Eqs A.41 into Eqs 9.35 gives: k−1

fcrN,k =

Fe,k,i Nc,i =

i=0 k−1

fcrM,k =

i=0

k−1

Fe,k,i ac0,i + ac1,i z

(9.36a)

Fe,k,i bc0,i + bc1,i z

(9.36b)

i=0

Fe,k,i Mc,i =

k−1 i=0

and the load vector accounting for creep is given as Eq. A.42. Similar to the inclusion of shrinkage effects in the AEMM, shrinkage is here included using: fshN = Ec,k εsh,k dA = Ec,k Ac εsh,k (9.37a) Ac

fshM =

Ac

yEc,k εsh,k dA = Ec,k Bc εsh,k

(9.37b)

9.6.3 Remarks on the consistency requirements for ﬁnite elements The proposed 7 DOF ﬁnite element represents the simplest element that fulﬁls the consistency requirements approximating the displacements by means of polynomials and thereby avoids potential locking problems which may arise when the member local z-axis does not pass through the centroid of the member cross-section (Refs 5 and 7). The ability to select a reference system with the origin not necessarily coincident with the centroid of the section is fundamental when dealing with time effects as the location of the actual centroid of a reinforced cross-section usually varies with time due to creep of the concrete. From a practical viewpoint, the consistency requirement is satisﬁed when the independent displacements (or their derivatives) present in the expressions of the strains of the model possess the same order (i.e. u and v have the same order). Adopting a cubic function for the deﬂection v produces a linear contribution to the

382 Stiffness method and ﬁnite-element modelling strain (i.e. due to v ). In order to produce the same (linear) contribution to the strain from u , it is necessary to have a parabolic function approximating the axial displacement u. For example, a linear function for u would not be able to achieve this as its ﬁrst derivative (i.e. u ) is constant. Other approaches could be used to address this problem, such as reduced integration. To better illustrate this behaviour, the results obtained using the 7 DOF ﬁnite element (Fig. 9.6) are compared to those calculated using a 6 DOF element (Fig. 9.7). The 6 DOF element approximates u and v by means of linear and cubic polynomials, respectively. As previously discussed, this latter element does not satisfy the consistency requirements due to the orders of its polynomials. The stiffness matrix of the 6 DOF ﬁnite element is: ⎤ ⎡ R R R R A B A B ⎥ ⎢ 0 − − 0 ⎢ L L L L ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ 12RI 6RI 12RI 6RI ⎥ ⎥ ⎢ 0 0 − 3 ⎥ ⎢ L3 L2 L L2 ⎥ ⎢ ⎥ ⎢ ⎢ R 6RI 4RI RB 6RI 2RI ⎥ ⎥ ⎢− B − 2 ⎥ ⎢ L L L L ⎥ L2 L (9.38) ke = ⎢ ⎥ ⎢ ⎥ ⎢ R RB RA RB ⎥ ⎢ A 0 0 − ⎥ ⎢− ⎢ L L L L ⎥ ⎥ ⎢ ⎢ 12RI 6RI 12RI 6RI ⎥ ⎥ ⎢ − 3 − 2 0 − 2 ⎥ ⎢ 0 3 ⎥ ⎢ L L L L ⎥ ⎢ ⎦ ⎣ RB 6RI 2RI RB 4RI 6RI − − L L L L L2 L2 For the case of an uncracked, simply supported, prismatic, concrete beam of rectangular section and subjected to a point load applied at mid-span, the instantaneous mid-span deﬂections calculated using the 6 and 7 DOF ﬁnite elements are shown in Fig. 9.8. These results have been obtained by considering two elements to clearly emphasise the implications of the different sets of polynomials. The instantaneous midspan deﬂection has been plotted for different levels of the reference axis dref (measured from the top of the section) expressed as a function of the depth D. With this notation the reference axis is located at the level of the centroid when dref /D = 0.5, in which case both elements produce the same mid-span deﬂection (noted as vmax in Fig. 9.8). Based on Fig. 9.8, it is apparent that when using the 6 DOF element with the origin of the reference system not coinciding with the cross-sectional centroid, a stiffer response than expected is obtained. A discussion on consistency requirements for different line elements is presented in Ref. 8. qR uL

qL vL

uR

vR

z L

Figure 9.7 Nodal displacements of the 6 DOF ﬁnite element.

Stiffness method and ﬁnite-element modelling 383

10%

vmax − vL/2 vmax [%]

8%

6 DOF element

6% 4% 2%

7 DOF element

dref D

0% 2

0

4

6

8

10

Figure 9.8 Comparisons between the results obtained using the 6 and 7 DOF ﬁnite elements.

Example 9.4 The short- and long-term values for the moment reaction at the ﬁxed support and the vertical reactions at the roller support of the propped cantilever shown in Fig. 9.9 are to be determined. The member is subjected to a point load applied at mid-span as shown. The time-dependent behaviour of the concrete is to be modelled using the AEMM and the cross-sectional and material properties are the same as in Example 5.3. For ease of notation, the beam is modelled using two of the 7 DOF line elements depicted in Fig. 9.6. 10 kN

B

1

2

A 10 m

C

10 m

Figure 9.9 Loading, support conditions and discretisation for Example 9.4.

The numbering of the freedoms adopted in the proposed solution is outlined in Fig. 9.10. The numbering system has been selected to produce the partitioning introduced in Eqs 9.8 and also to avoid the need for transformations from local to global coordinates (as the local and global coordinate axes coincide for each element). 1 10

2 C

B

A 9 11

7

2

1 3

4

8

5 6

Figure 9.10 Freedom numbering for Example 9.4.

384 Stiffness method and ﬁnite-element modelling From Examples 5.1 and 5.3: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 RA,k = 2175 × 106 N RB,k = 273.7 × 109 Nmm RI,k = 113.2 × 1012 Nmm2 Ec,0 = 25,000 MPa Ee,k = 9524 MPa Fe,0 = −0.333 ϕ(τk , τ0 ) = 2.5 χ(τk , τ0 ) = 0.65 εsh (τk ) = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4

Instantaneous analysis (at time τ0 ) Based on Fig. 9.10, freedoms 1–7 are unrestrained, while no displacement is permitted for each of freedoms 8–11. Therefore: T UU,0 = U1,0 U2,0 U3,0 U4,0 U5,0 U6,0 U7,0 T T UK,0 = U8,0 U9,0 U10,0 U11,0 = 0 0 0 0 T PU,0 = P8,0 P9,0 P10,0 P11,0 The ﬁnite-element stiffness matrix ke,0 is identical for both elements 1 and 2 and is calculated at time τ0 substituting RA,0 , RB,0 and RI,0 into Eq. 9.28 and specifying an element length L equal to 10 × 103 mm. The stiffness matrix of the whole structure is then assembled following similar steps to those carried out in previous examples. The unknown displacements and reactions are calculated using Eqs 9.9: ⎡ ⎤ 0.021 mm ⎢ ⎥ ⎤ ⎡ ⎡ ⎤ ⎢ 4.531 mm ⎥ ⎢ ⎥ −3125 N P8,0 −6 ⎢ 194.2 × 10 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ P9,0 ⎥ ⎢ 0N ⎥ ⎥ and PU,0 = ⎢ UU,0 = ⎢ = ⎥ ⎢ ⎢ ⎥ −0.059 mm ⎢ ⎥ ⎣P10,0 ⎦ ⎣ ⎦ −6875 N ⎢ ⎥ ⎢ −0.085 mm ⎥ 6 ⎢ ⎥ −37.5 × 10 Nmm P11,0 ⎣−776.7 × 10−6 ⎦ 0.070 mm

Stiffness method and ﬁnite-element modelling 385 The moment reaction at the ﬁxed support (related to freedom 11) and the vertical reaction at the roller support (related to freedom 8) are equal to −37.5 kNm and −3125 N, respectively.

Post-processing The solution is now post-processed to determine the coefﬁcients describing the variation of the concrete stress resultants required subsequently to account for creep effects. The nodal displacements for elements 1 and 2 at time τ0 are collected in vectors u(1),0 and u(2),0 : ⎡

⎤

uL(1),0

⎡

0 mm

⎤

⎤

⎡ uL(2),0

⎡

0.021 mm

⎥ ⎥ ⎢ ⎢ ⎥ ⎢vL(1),0⎥ ⎢ ⎢ vL(2),0 ⎥ ⎢ ⎥ 0 mm 4.531 mm ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎢ ⎥ ⎢ 194.2 × 10−6 v ⎥ ⎢vL(1),0⎥ ⎢ ⎢ 0 ⎥ ⎥ ⎢ ⎢ ⎢ L(2),0 ⎥ ⎢ ⎥ = ⎢ 0.070 mm ⎥ ⎥ ⎢ −0.059 mm ⎢u u(1),0 = ⎢ and u = ⎥ u (2),0 ⎢ M(1),0⎥ ⎢ ⎢ M(2),0 ⎥ = ⎢ ⎥ ⎥ ⎥ ⎢ ⎢ ⎢ ⎢uR(1),0⎥ ⎢ ⎢ uR(2),0 ⎥ ⎢ −0.085 mm 0.021 mm ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ⎣ 4.531 mm ⎥ ⎥ ⎢ ⎢v ⎢v ⎦ ⎣ 0 mm ⎣ R(1),0⎦ ⎣ R(2),0 ⎦ vR(1),0

194.2 × 10−6

vL(2),0

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦

−776.7 × 10−6

and from Eqs A.35: ac0(1),0 = 12.56 × 103 Nmm2 ac1(1),0 = −2.304 Nmm−1 bc0(1),0 = −29.34 × 106 Nmm bc1(1),0 = 5.379 × 103 N ac0(2),0 = −10.47 × 103 Nmm2 ac1(2),0 = 1.047 Nmm−1 bc0(2),0 = 24.45 × 106 Nmm bc1(2),0 = −2.45 × 103 N

Long-term analysis (at time τk ) The unknown and known displacements at time τk and the unknown reactions are: T UU,k = U1,k U2,k U3,k U4,k U5,k U6,k U7,k T T UK,k = U8,k U9,k U10,k U11,k = 0 0 0 0 T PU,k = P8,k P9,k P10,k P11,k

386 Stiffness method and ﬁnite-element modelling The ﬁnite-element stiffness matrix ke,k for elements 1 and 2 is obtained from Eq. 9.28 using the cross-sectional properties RA,k , RB,k and RI,k . The load vectors accounting for shrinkage effects for both elements 1 and 2 are calculated at time τk using Eq. A.37: ⎡ ⎤ 1015 × 103 N ⎢ ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢−99.79 × 106 Nmm⎥ ⎢ ⎥ ⎢ ⎥ pe.sh(1),k = pe.sh(2),k = ⎢ ⎥ 0N ⎢ ⎥ ⎢ −1015 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ ⎦ 0N 99.79 × 106 Nmm The vectors describing the creep effects for elements 1 and 2 are calculated from Eq. A.36 using the coefﬁcient acj(i),0 and bcj(i),0 stored at the end of the instantaneous analysis: ⎤ ⎡ ⎡ ⎤ 2909 N −2909 N ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ 1793 N −815.0 N ⎥ ⎢ ⎢ ⎥ ⎢9779 × 103 Nmm⎥ ⎢−8150 × 103 Nmm⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ pe.cr(1),k = ⎢ ⎥ ⎥ and pe.cr(2),k = ⎢ −5119 N 2327 N ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ 2211 N 581.7 N ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎦ ⎣ ⎣ ⎦ −1793 N 815.0 N 8150 × 103 Nmm

0 Nmm

The unknown displacements and reaction are then obtained using Eqs 9.9 following assembly of the global stiffness matrix and load vector (as was previously carried out at time τ0 ): ⎡ ⎤ −4.544 mm ⎢ ⎥ ⎤ ⎡ ⎡ ⎤ ⎢ 19.22 mm ⎥ ⎢ ⎥ −1033 N P 8,k ⎢ 948.3 × 10−6 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ P9,k ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ UU,k = ⎢ −7.219 mm ⎥ and PU,k = ⎢ =⎢ ⎥ ⎥ ⎢ ⎥ −8967 N P ⎦ ⎣ ⎣ ⎦ 10,k ⎢ −9.814 mm ⎥ ⎢ ⎥ 6 −79.35 × 10 Nmm P11,k ⎢ ⎥ ⎣−3.793 × 10−3 ⎦ −2.051 mm The moment reaction at the ﬁxed support (related to freedom 11) and the vertical reaction at the roller support (related to freedom 8) are equal to −79.35 kNm and −1033 N, respectively. For this lightly loaded member, the preponderance of reinforcement in the bottom ﬁbres has caused the redistribution of internal actions illustrated in Fig. 8.5b(i).

Stiffness method and ﬁnite-element modelling 387

9.7 Analysis of cracked members A realistic analysis of concrete structures needs to account for the effects of cracking of the concrete. This is certainly important for calculations carried out at service conditions where signiﬁcant errors in the evaluation of deformations and stresses will arise if the effects of cracking are not included. In Chapter 7, cracking of the concrete is included in the cross-sectional analysis in one of two ways. In the ﬁrst more approximate approach, the extent of cracking is determined from the instantaneous analysis assuming the concrete can carry no tension and, for the time analysis, the extent of cracking and the depth of the intact concrete on the cross-section are assumed to remain unchanged. The second approach to the time analysis of a cracked cross-section is a more reﬁned method of analysis that traces the crack development with time by accounting for the change in the depth of the concrete compressive zone as time progresses. This latter approach is particularly suitable for the analysis and design of structural members where deﬂection or crack control at the serviceability limit states are the governing design considerations. In the following, the application of these two approaches using the stiffness method and the ﬁnite-element approach is discussed. More advanced non-linear software for modelling cracking in concrete structures is available, but the two proposed methods provide a practical balance between the complexity adopted in the analysis and the variability of the concrete properties required for input into the analysis. 9.7.1 Approach 1 Cracking occurs when the stresses in the concrete produced by applied loads or deformations reach the tensile strength of the concrete. In the case of statically indeterminate members, the internal actions at a particular cross-section depend on the extent of cracking and this is usually unknown at the beginning of the analysis. A simple and practical method for including cracking in the analysis of a structure involves an iterative procedure that is illustrated here by considering the propped cantilever shown in Fig. 9.11. The ﬁrst iteration involves the analysis of the structure using either the stiffness or ﬁnite-element methods assuming the whole structure to be uncracked (Fig. 9.11b) following the procedures presented in the previous sections. Based on these results, the extent of cracking to be used in the second iteration is determined. In the propped cantilever of Fig. 9.11c, cracking occurs in that part of the beam adjacent to the ﬁxed support where the applied moment is greater than the cracking moment Mcr (where Mcr was introduced in Chapter 3 and is the moment required to produce an extreme ﬁbre tensile stress in the concrete equal to its tensile strength). The cross-sectional properties of the cracked region are next obtained following the procedure presented in Chapter 7 and the member is then re-analysed using the revised cross-sectional rigidities. At the end of the second iteration, the lengths of the cracked and uncracked segments are adjusted based on the revised bending moment diagram, as shown in Fig. 9.11d, and the updated stiffnesses are adopted for the third iteration. The adjustments of the cracked and uncracked lengths continue until two subsequent iterations produce negligible differences. The implementation of the convergence criteria can be carried out in different ways depending on the modelling technique adopted. For example, the beam shown in

388 Stiffness method and ﬁnite-element modelling

(a) Support and loading arrangements.

Uncracked (b) Iteration 1: Uncracked length and bending moment diagram. Mcr Mcr

M

Cracked

Uncracked

(c) Iteration 2: Cracked and uncracked segments and bending moment diagram Mcr Mcr M Cracked Uncracked

Cracked Uncracked

(d) Iteration 3: Cracked and uncracked segments and bending moment diagram.

Mcr Mcr M

Figure 9.11 First iterations of the analysis of a propped cantilever using approach 1.

Fig. 9.11 could be modelled using different stiffness (or ﬁnite) elements for each cracked and uncracked region. The lengths of the cracked and uncracked segments would change from iteration to iteration. Convergence is achieved when the required adjustments of lengths for each segment is negligible. This approach can be applied only for simple members, such as the one shown in Fig. 9.11, as its use becomes prohibitive for large systems. In the case of more complex structures, it is preferable to discretise the whole structure using a predeﬁned element mesh and to assign to each element either cracked or uncracked properties based on the calculated internal actions. In this case, the ﬁrst iteration is also carried out assuming all elements are uncracked. After the instantaneous solution at time τ0 is completed, the time analysis is carried out assuming

Stiffness method and ﬁnite-element modelling 389 the extent of the cracked and uncracked regions does not change with time. For this purpose, the use of the AEMM to determine the time-dependent behaviour is recommended. In this way, only one additional analysis is required with no further iterations. Clearly, the method does not account for time-dependent cracking, as no attempt is made to discretise the time domain. This method is suitable for modelling structures when only linear-elastic analysis software is available. 9.7.2 Approach 2 The main advantage of this second approach relies on its ability to follow the occurrence and development of cracking throughout the structure. This is particularly useful for structural elements recognised to be critical at service conditions. In the more reﬁned, second approach, the structure is discretised into a predetermined layout of elements, with the number and size of elements selected depending on the degree of accuracy required. The extent of initial cracking in the structure is then determined by performing a non-linear analysis at time τ0 . This is usually based on well-known non-linear solution strategies such as the secant or Newthon–Raphson methods. Both can be implemented with the stiffness and ﬁnite element methods, even if the latter is naturally more suitable for these types of analysis. In fact, when using the ﬁnite element approach to analyse a concrete structure, the non-linear response of the concrete is accounted for in the numerical integration of the stiffness coefﬁcients and of the load vectors. Considering the line element shown in Fig. 9.6, these approximations are applied to the integrals of Eqs A.25 and A.26 following procedures well established for the ﬁnite element method (Refs 2 and 4). In this process, the section is subdivided into smaller areas in order to better depict the non-linear response, such as the layered cross-sections already discussed in Section 7.4. With the stiffness method, the appropriate cross-sectional rigidities are calculated at one or more locations along the member length following the approach presented in Chapter 7. When the instantaneous analysis is completed, the time analysis is carried out by discretising the time domain into a number of steps and modelling the concrete behaviour using the SSM. With this approach, the time-dependent behaviour of the concrete is carefully monitored at the integration points along each element. The main non-linearity addressed in this analysis originates from the fact that the concrete is assumed not to be able to carry tensile stresses greater than its tensile strength. If at any time instant the concrete stress at any calculation point exceeds the tensile strength, the previously stored stress history at this point is set to zero, the contribution to element stiffness is adjusted and the structure is reanalysed. The process continues until no new cracking is identiﬁed at any point in the structure. Of course, if a cracked point is later subjected to compressive stresses during subsequent time steps, the point again becomes active and contributes to the element stiffness. Obviously, tension-stiffening could also be included in the analysis, even if its time-dependent behaviour is still the focus of current research (Ref. 6).

9.8 References 1. Hibbeler, R.C. (2009). Structural Analysis. Seventh edition, Pearson Prentice Hall. 2. Bathe, K.J. (2006). Finite Element Procedures. Prentice Hall, New Jersey.

390 Stiffness method and ﬁnite-element modelling 3. Weaver, W. and Gere, J.M. (1990). Matrix Analysis of Framed Structures. Third edition, Van Nostrand Reinhold, New York. 4. CEB-FIB (2008). Practitioners’ Guide to Finite Element Modelling of Reinforced Concrete Structures. International Federation for Structural Concrete, ﬁb Bulletin 45, Lausanne, Switzerland. 5. Crisﬁeld, M.A. (1991). The eccentricity issue in the design of plate and shell elements. Communications in Applied Numerical Methods, 7, 47–56. 6. Gilbert, R.I. and Wu, H.Q. (2009). Time-dependent stiffness of cracked reinforced concrete elements under sustained actions. Australian Journal of Structural Engineering, Engineers Australia, 9(2) 151–158. 7. Gupta, A.K. and Ma, P.S. (1977). Error in eccentric beam formulation. International Journal for Numerical Methods in Engineering, 11, 1473–1483. 8. Ranzi, G. and Zona, A. (2007). A composite beam model including the shear deformability of the steel component. Engineering Structures, 29, 3026–3041.

Appendix A Analytical formulations Euler–Bernoulli beam model

A.1 Introduction The Euler–Bernoulli beam model is widely used for the analysis of structures. Designers use it on a daily basis in the form of either closed form solutions, such as those provided for the estimate of elastic deﬂections, or line (frame) elements for the prediction of deformations and internal actions using commercial structural analysis software. The analytical formulation at the basis of the Euler–Bernoulli beam model is described in the following sections for generic concrete members (such as those shown in Fig. A.1), where a perfect bond is assumed between the concrete and the reinforcement. The weak form of the model (global balance condition) is presented to provide a basis for the ﬁnite element formulation brieﬂy introduced in Chapter 9. The strong form (local balance condition) is then obtained by integrating this by parts. This has been used to derive the stiffness matrix and equivalent nodal actions required for the stiffness method described in Chapter 9. The proposed formulations are derived for a typical instant in time and, because of this, could be applicable to both short- and long-term analyses. For ease of notation, additional subscripts are included in this appendix to identify the time step under

z

L x y

(a) Reinforced concrete beam

z

L x y

(b) Prestressed concrete beam

Figure A.1 Typical concrete members and cross-sections.

392 Analytical formulations consideration only when it may not be clear from the context. A similar approach is used when deﬁning the time dependency of variables. For example, the deﬂection along the member length that is a function of both member coordinate z and time t will be referred to as v(z) (or simply v) instead of v(t, z).

A.2 Kinematic model In the undeformed state, the beam is assumed to be prismatic with the ortho-normal reference axis system {O; x, y, z} as shown in Fig. A.1. The kinematic behaviour is illustrated in Fig. A.2b for a generic point P on the z-axis, highlighting both its axial displacement at the level of the reference axis u(z) and its deﬂection v(z). The formulation is derived for a beam segment of length L and the cross-section is assumed to be symmetric about the y-axis. Under these assumptions, no torsional and out-of-plane ﬂexural effects are considered. The level of the reference x-axis is arbitrary. Considering a point Q located away from the member axis, its ﬁnal displacement can be expressed in terms of u(z) and v(z) as well as the rotation θ(z). In particular, the vertical and horizontal displacements, referred to as dy (y, z) and dz (y, z), can be expressed as: dy (y, z) = v (z) − y + y cos θ (z)

(A.1a)

dz (y, z) = u (z) − y sin θ (z)

(A.1b)

and, for clarity, the kinematic response of the point Q is illustrated in Fig. A.2c. The expressions of Eqs A.1 describe all possible displacements that the points of the beam can undergo. This set of displacements is usually referred to as the displacement ﬁeld of the model. For structural engineering applications, it is usually sufﬁcient and z

P L Elevation

y

Section

(a ) P

u(z)

P

z yQ

v(z)

z dz(y, z)

Q

y

y dy(y, z)

(b)

P′

q(z)

q(z)

(c)

P′

yQcos(q(z)) yQsin(q(z))

Figure A.2 Displacement ﬁeld.

Q′

Analytical formulations 393 convenient to remain within the framework of small displacements. In this way, the cosine and sine of the angle θ(z) in Eqs A.1 can be approximated by: cos θ(z) ≈ 1 and sin θ(z) ≈ θ(z). Consistent with the assumptions of the Euler-Bernoulli beam model, plane sections are assumed to remain plane and perpendicular to the beam axis before and after deformations. This condition implies that: θ (z) = v (z)

(A.2)

where the prime represents differentiation with respect to z. Based on these simpliﬁcations the displacement ﬁeld of Eqs A.1 can be re-written as: dy (y, z) = v (z)

(A.3a)

dz (y, z) = u (z) − y θ (z) = u (z) − yv (z)

(A.3b)

Equations A.3 show how the kinematic response of a point in the beam can be determined when the displacements u(z) and v(z) are known. For ease of notation, u(z), v(z) and θ(z) will be referred to as u, v and θ, respectively, in the following. Based on the adopted displacement ﬁeld, the only non zero strain is: εz = u − yv

(A.4)

where εz is the axial strain of the member. The expression for the curvature κ(= −v ) can be obtained by differentiating the deﬂection v twice with respect to the coordinate z, and the negative sign in front of v is required in ﬂexural members to produce a positive curvature in sagging moment regions (i.e. where compressive and tensile strains occur in the top and bottom ﬁbres of the section in a horizontal beam, respectively, in accordance with the sign convention adopted in this book).

A.3 Weak formulation (global balance condition) The weak form of the structural formulation for the frame element is obtained using the principle of virtual work considering a beam segment of length L with the free body diagram shown in Fig. A.3. In particular, p(z) and n(z) represent the vertical and horizontal distributed member loads which, for ease of notation, will be referred to as p and n in the following. The nodal actions at each end of the member represent external loads or reactions depending on the boundary conditions of the beam segment and have been referred to as S, N and M with the subscripts L and R specifying whether they relate to the left (at z = 0) or right (at z = L) ends of the member, respectively, as shown in Fig. A.3. The derivation is carried out by equating the work of internal stresses to the work of external actions for each virtual admissible variation of the displacements and corresponding strains (which, by deﬁnition, represent all variations of

394 Analytical formulations p(z) MR

ML NL

NR

n(z) SL

SR

z L

Figure A.3 Member loads and nodal actions.

possible displacements satisfying the kinematic boundary conditions of the problem) as follows: σz εˆ z dA dz = pˆv +nuˆ dz +SL vˆ L +NL uˆ L +ML θˆL +SR vˆ R +NR uˆ R +MR θˆR L A

L

(A.5)

where the variables with the hat ‘ˆ’ represent virtual variations of displacements or strains. Substituting the expression for the axial strain εz of Eq. A.4 into Eq. A.5, the weak form of the derivation can be re-written as: pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL σz uˆ − yˆv dA dz = L A

L

+ SR vˆ R + NR uˆ R + MR θˆR

(A.6)

Recalling the deﬁnitions of internal axial force N and moment M (about the x-axis) introduced in Chapter 5 and reproduced here for ease of reference: Ni =

A

σz dA

and

Mi =

A

yσz dA

(A.7a,b)

the integral at the cross-section (i.e. in dA) present on the left-hand side of Eq. A.6 can be replaced by these internal actions as: L

Ni uˆ − Mi vˆ dz =

L

pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL

+ SR vˆ R + NR uˆ R + MR θˆR

(A.8)

This relationship can be further rearranged to isolate the terms related to Ni and Mi as follows: ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ vˆ L SR vˆ R SL Ni uˆ n uˆ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ · dz = · dz + ⎣ NL ⎦ · ⎣uˆ L ⎦ + ⎣ NR ⎦ · ⎣uˆ R ⎦ Mi −ˆv vˆ L p ML θˆL MR θˆR

L

(A.9)

Analytical formulations 395 It is possible to ignore the nodal actions included on the right-hand side of Eq. A.9 as these can be easily included in the frame analysis during the assembly of the load vector. Based on this, Eq. A.9 can be simpliﬁed to: L

Ni uˆ n uˆ · dz = · dz Mi −ˆv vˆ L p

(A.10)

In this form, the constitutive models for the materials are not explicitly speciﬁed as they are included in the deﬁnitions of the internal actions Ni and Mi . To remain consistent with the notation adopted in the rest of the book, the expressions already introduced in Chapter 5 (reproduced here for ease of reference) are adopted in the following to deﬁne the internal actions as a function of the material properties: ri = Dε + fcr − fsh

(A.11)

which can be written highlighting the terms included in the matrix and vectors as: RA Ni = Mi RB

RB RI

εr κ

+

fcrN

fcrM

−

fshN

(A.12)

fshM

and the cross-sectional rigidities RA , RB and RI are deﬁned in Chapter 5 for different types of cross-sections. In particular, ri collects the internal axial force Ni and internal moment Mi , D speciﬁes the geometric and material properties of the cross-section, ε includes the strain calculated at the level of the reference axis εr and the curvature κ which can be expressed in terms of the horizontal and vertical displacements (i.e. u and v) as shown below, while f cr and f sh account for creep and shrinkage effects, respectively: 1 Ni σz dA RA A = 1 ; D= ri = Mi yσ dA RB z A f f fcr = crN and fsh = shN fcrM fshM

RB RI

;

ε=

εr κ

u = −v

(A.13a,b,c)

(A.13d,e)

This representation of f cr and f sh is particularly useful as it enables the proposed derivation to be applicable when using either the age-adjusted effective modulus method (AEMM) or the step-by-step method (SSM). When using the AEMM the components of f cr and f sh are determined as: fcrN =

Ac

fcrM =

Ac

Fe,0 σc,0 dA = Fe,0 Nc,0 Fe,0 yσc,0 dA = Fe,0 Mc,0

and fshN = Ee,k Ac εsh,k and fshM = Ee,k Bc εsh,k

(A.14a,b) (A.14c,d)

396 Analytical formulations where Ee,k and Fe,0 are deﬁned in Eqs 4.35 and 4.46. When using the SSM, these components at time τk become: fcrN =

fcrM =

k−1 i=0 Ac k−1 i=0 Ac

k−1

Fe,k,i σc,i dA =

Fe,k,i Nc,i and fshN = Ec,k Ac εsh,k

(A.15a,b)

i=0

Fe,k,i yσc,i dA =

k−1

Fe,k,i Mc,i and fshM = Ec,k Bc εsh,k

(A.15c,d)

i=0

where σc,i is the stress in the concrete at time τi , while Nc,i and Mc,i represent the axial force and moment, respectively, resisted by the concrete component at time τi . The vector ε can also be re-written in terms of the independent displacements u and v as: ε=

εr κ

u ∂ 0 u = = = Ae 2 −v 0 −∂ v

(A.16)

where A is a differential operator and the symbol ∂ deﬁnes the derivative with respect to the member coordinate z and the displacements u and v are collected in vector e as: u e= v

(A.17)

At this point it is useful to re-write Eq. A.10 in terms of vectors ri and ε (= A e): L

ri · A eˆ dz =

L

q · eˆ dz

(A.18)

where the member loads n and p have been collected in the vector q as: q=

n

(A.19a,b)

p

Substituting the constitutive properties deﬁned in Eq. A.11 into Eq. A.18 produces the general expression for the weak form accounting for time effects: L

Dε + fcr − fsh · A eˆ dz =

L

q · eˆ dz

(A.20)

A.4 Finite element formulation The formulation proposed in the following is applicable to displacement-based ﬁnite elements. If necessary, the approach can be extended to other elements, i.e. forcebased or mixed elements. The basis of the ﬁnite element formulation relies on the

Analytical formulations 397 approximation of the independent displacements u and v, previously collected in the vector e. This approximation can be expressed as: e∼ = N e de

(A.21)

in which Ne is the matrix that speciﬁes the adopted shape functions and de is the vector of the nodal displacements of the ﬁnite element. Substituting the approximation of Eq. A.21 into Eq. A.20 produces the weak form of the problem expressed in terms of nodal displacements: L

Dε + fcr − fsh · A Ne dˆ e dz =

L

q · Ne dˆ e dz

(A.22)

This relationship can be re-arranged to isolate the virtual nodal displacements dˆ e on one side of the dot product: L

(A Ne )T Dε + fcr − fsh dz · dˆ e =

L

NeT q dz · dˆ e

(A.23)

from which the stiffness relationship of the ﬁnite element can be obtained: ke de = pe

(A.24)

where ke is the ﬁnite element stiffness matrix and pe represents the loading vector related to both member loads and time effects. In particular, these are deﬁned as: ke =

L

(A Ne )T D ε dz =

L

(A Ne )T D (A Ne ) dz

(A.25a)

pe = pe.m − pe.cr + pe.sh

(A.25b)

where the loading vector pe has been separated into pe.m , pe.cr , and pe.sh relating to member loads (n and p), creep effects and shrinkage effects, respectively, and given by: pe.m =

L

NeT q

dz;

pe.cr =

T

L

(A Ne ) fcr dz;

and pe.sh =

L

(A Ne )T fsh dz (A.26a–c)

Conventional ﬁnite element procedures are then utilized to assemble the vectors and matrices for the whole structure and to perform the structural analysis (Refs 1 and 2). The derivations are outlined in the following by means of worked examples. A.4.1 Age-adjusted effective modulus method Expressions for the stiffness matrix and loading vectors related to member loads, creep effects and shrinkage effects for the 7 DOF ﬁnite element shown in Fig. 9.6 are derived here. For this element, the axial (u) and transverse displacements (v) are approximated using parabolic and cubic functions, respectively. The time-dependent behaviour of the

398 Analytical formulations concrete is modelled using the AEMM speciﬁed in Eq. 4.45 (Approach 2 in Section 4.4.4). The parabolic and cubic approximation for the axial and vertical displacements of the 7 dof element are: u = Nu1 uL + Nu2 uM + Nu3 uR

and v = Nv1 vL + Nv2 θL + Nv3 vR + Nv4 θR (A.27a,b)

where: Nu1 = 1 −

3z 2z2 + 2; L L

Nv1 = 1 −

3z2 2z3 + 3; L2 L

3z2 2z3 − 3; L2 L

Nv3 =

Nu2 =

4z 4z2 − 2; L L

Nv2 = z −

Nv4 = −

Nu3 = −

z 2z2 + 2 L L

(A.28a–c)

2z2 z3 + 2; L L

(A.29a,b)

z2 z3 + L L2

(A.29c,d)

It is usually convenient to represent these approximations by means of the matrix of shape functions Ne and a vector de collecting the nodal displacements: ⎤ uL ⎢ ⎥ ⎢ vL ⎥ ⎢ ⎥ ⎢ θ ⎥ ⎢ L⎥ 0 ⎢ ⎥ ⎢uM ⎥ = Ne de ⎥ Nv4 ⎢ ⎢u ⎥ ⎢ R⎥ ⎢ ⎥ ⎣ vR ⎦ ⎡

u v

=

Nu1 0

0

0

Nu2

Nu3

0

Nv1

Nv2

0

0

Nv3

(A.30)

θR The stiffness matrix of the 7 DOF ﬁnite element can be calculated based on Eq. A.25a. This requires the calculation of A Ne which, recalling the deﬁnition of the differential operator A speciﬁed in Eq. A.16, is obtained as: ⎡

A Ne

N = ⎣ u1 0

⎡

0

0

−Nv1

−Nv2

⎢− 3 + 4z ⎢ L L2 =⎢ ⎢ ⎣ 0

Nu2

0

⎤

Nu3

0

0

−Nv3

0

0

12z 6 − 3 L2 L

4 6z − L L2

0 ⎦ −Nv4

⎤

4 8z 1 4z − + 2 − L L2 L L 0

0

0 −

6 12z + 3 L2 L

0

⎥ ⎥ ⎥ ⎥ 6z ⎦

2 − L L2

Analytical formulations 399 Substituting the expression obtained for A Ne into Eq. A.25a and carrying out the integration along the member length produces the element stiffness matrix: ⎡ ⎢ 7RA ⎢ 3L ⎢ ⎢ ⎢ −4RB ⎢ ⎢ L2 ⎢ ⎢ ⎢ −3RB ⎢ ⎢ ⎢ L ⎢ ⎢ ke = ⎢ −8RA ⎢ ⎢ 3L ⎢ ⎢ R ⎢ A ⎢ ⎢ 3L ⎢ ⎢ ⎢ 4RB ⎢ ⎢ L2 ⎢ ⎣ −RB L

−4RB L2

−3RB L

−8RA 3L

RA 3L

4RB L2

12RI L3

6RI L2

8RB L2

−4RB L2

−12RI L3

6RI L2

4RI L

4RB L

−RB L

−6RI L2

8RB L2

4RB L

16RA 3L

−8RA 3L

−8RB L2

−4RB L2

−RB L

−8RA 3L

7RA 3L

4RB L2

−12RI L3

−6RI L2

−8RB L2

4RB L2

12RI L3

6RI L2

2RI L

4RB L

−3RB L

−6RI L2

⎤ −RB ⎥ L ⎥ ⎥ ⎥ 6RI ⎥ ⎥ L2 ⎥ ⎥ ⎥ 2RI ⎥ ⎥ ⎥ L ⎥ ⎥ 4RB ⎥ ⎥ ⎥ L ⎥ ⎥ −3RB ⎥ ⎥ ⎥ L ⎥ ⎥ ⎥ −6RI ⎥ ⎥ L2 ⎥ ⎥ ⎦ 4RI L

(A.31)

Recalling the expression previously obtained for A Ne , the loading vectors are then calculated based on Eqs A.26. In particular, the one related to the member loads n and p can be derived as: ⎡

⎡ Nu1 ⎢ ⎢ 0 ⎢ ⎢ ⎢ 0 ⎢ pe.m = NeT q dz = ⎢ ⎢Nu2 L L⎢ ⎢Nu3 ⎢ ⎢ ⎣ 0 0

⎤ L ⎢ ⎥ ⎢ 6n ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ L ⎥ ⎢ ⎤ p ⎥ ⎢ ⎥ 2 ⎢ ⎥ 0 ⎢ ⎥ ⎥ ⎢ ⎥ 2 L Nv1 ⎥ ⎢ ⎥ ⎥ p ⎢ ⎥ ⎥ 12 ⎢ ⎥ Nv2 ⎥ ⎢ ⎥ ⎥ n ⎢ ⎥ ⎥ 2L dz = ⎢ ⎥ 0 ⎥ n ⎢ ⎥ p ⎥ ⎢ ⎥ 3 0 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎥ L ⎢ ⎥ Nv3 ⎦ n ⎥ ⎢ ⎢ 6 ⎥ ⎢ ⎥ Nv4 ⎢ ⎥ ⎢ L ⎥ ⎢ p ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎣ ⎦ L2 − p 12

(A.32)

As highlighted in Eq. A.26b, the calculation of the loading vector describing creep effects pe.cr requires the knowledge of the axial force and moment for the calculation of fcrN and fcrM included in f cr . These depend to the loading history of the concrete as

400 Analytical formulations both fcrN and fcrM are determined by multiplying the axial force and moment resisted by the concrete at one or more instants in time by particular material coefﬁcients. The deﬁnition of these coefﬁcients varies depending on the constitutive relationship for concrete and, for the AEMM, it is given in Eqs A.14. The analysis at a particular instant in time can be carried out only if the instantaneous analysis has been completed and the concrete stress resultants recorded. The actual recording of these actions can be carried out by storing the values of the concrete axial force and moment at particular locations along each member. These locations are usually those required by the numerical integration of Eq. A.26b. Another option is to identify polynomials capable of describing the variation of the concrete axial force and moment along each element and to store the relevant coefﬁcients. This option is preferred here as it enables closed form solutions to be obtained. The orders of the polynomial describing fcrN and fcrM (Eqs A.14) depend on the orders of the expressions for the axial force and moment resisted by the concrete at time τ0 , Nc.0 and Mc.0 . Recalling that: σc,0 dA = Ec,0 u0 − yv0 dA = Ac Ec,0 u0 − Bc Ec,0 v0 (A.33a) Nc,0 = Ac

Ac

Mc,0 =

Ac

yσc,0 dA =

Ac

yEc,0 u0 − yv0 dA = Bc Ec,0 u0 − Ic Ec,0 v0

(A.33b)

and considering that, in the 7 DOF ﬁnite element (Fig. 9.6), u and v are approximated by a parabolic and a cubic polynomial, respectively, the actual functions describing Nc,0 and Mc,0 determined using Eqs A.33 become linear and can be expressed as: Nc.0 = ac0,0 + ac1,0 z

and Mc.0 = bc0,0 + bc1,0 z

where the coefﬁcients ac0,0 , ac1,0 , bc0,0 , and bc1,0 are determined from Eqs A.33. Considering Eqs A.27–A.30, the expressions for u0 and v0 can be written in terms of the nodal displacements of the ﬁnite element as: uL,0 +Nu2 uM,0 +Nu3 uR,0 u0 = Nu1

3 4z 4 8z 1 4z = − + 2 uL,0 + uM,0 + − + 2 uR,0 − L L L L2 L L

3 4 1 4 8 4 = − uL,0 + uM,0 − uR,0 + uL,0 − 2 uM,0 + 2 uR,0 z L L L L2 L L

(A.34a)

v0 = Nv1 vL,0 +Nv2 θL,0 +Nv3 vR,0 +Nv4 θR,0

6 12z 4 6z 6 12z 2 6z = − 2 + 3 vL,0 + − + 2 θL,0 + − v + − θR,0 + R,0 L L L L2 L L L2 L 3

6 4 6 2 12 6 12 6 = − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 + 3 vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z L L L L L L L L (A.34b)

The ‘0’ subscript in the nodal freedoms in Eqs A34 is to specify that these are calculated at time τ0 .

Analytical formulations 401 The expression for the concrete axial force Nc,0 can then be obtained by substituting Eqs A.34 into Eq. A.33a:

Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0

3 4 1 4 8 4 = Ac Ec,0 − uL,0 + uM,0 − uR,0 + u − u + u L,0 M,0 R,0 z L L L L2 L2 L2

6 4 6 2 − Bc Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

12 6 12 6 + vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z 3 L L L L = ac0,0 + ac1,0 z

(A.35a)

where:

3 4 1 ac0,0 = Ac Ec,0 − uL,0 + uM,0 − uR,0 L L L

6 4 6 2 − Bc Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

4 8 4 ac1,0 = Ac Ec,0 uL,0 − 2 uM,0 + 2 uR,0 L2 L L

12 6 12 6 − Bc Ec,0 v + θ − v + θ L,0 L,0 R,0 R,0 L3 L2 L3 L2

(A.35b)

(A.35c)

Similarly, substituting Eqs A.34 into Eq. A.33b leads to the expression for Mc,0 :

Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0

3 4 1 4 8 4 = Bc Ec,0 − uL,0 + uM,0 − uR,0 + z u − u + u L,0 M,0 R,0 L L L L2 L2 L2

6 4 6 2 − Ic Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

12 6 12 6 + vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z L3 L L L = bc0,0 + bc1,0 z

(A.35d)

402 Analytical formulations where:

3 4 1 bc0,0 = Bc Ec,0 − uL,0 + uM,0 − uR,0 L L L

6 4 6 2 − Ic Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

4 8 4 bc1,0 = Bc Ec,0 uL,0 − 2 uM,0 + 2 uR,0 2 L L L

12 6 12 6 − Ic Ec,0 vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 L3 L L L

(A.35e)

(A.35f)

At this point, it is possible to derive the expressions for fcrN and fcrM substituting Eqs A.35 into Eqs A.14a and c: Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z fcrN = fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z and pe.cr can then be obtained as follows: pe.cr = (A Ne )T fcr dz L

⎡

⎤

⎢− 3 + 4z2 ⎢ L L

⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ = ⎢ 4 − 8z L⎢ ⎢ L L2 ⎢ 1 4z ⎢− + ⎢ L L2 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎣ 0

⎥ ⎥ ⎡ ⎤ ⎥ L −ac0,0 − ac1,0 12z ⎥ 6 6 − 3 ⎥ ⎢ ⎥ L2 L ⎥ ⎢ ⎥ ⎥ −b c1,0 ⎢ ⎥ ⎢ ⎥ 4 6z ⎥ − 2 ⎥ ⎢ ⎥ b c0,0 L L ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ F a + a z ⎥ e,0 c0,0 2 c1,0 ⎢ dz = Fe,0 ⎢ − Lac1,0 ⎥ ⎥ ⎥ 0 ⎥ 3 ⎢ ⎥ ⎥ Fe,0 bc0,0 + bc1,0 z 5 ⎢ ⎥ ⎥ La + a ⎢ ⎥ c1,0 c0,0 ⎥ ⎢6 ⎥ 0 ⎥ ⎢ ⎥ ⎥ ⎣ ⎦ bc1,0 ⎥ 12z ⎥ 6 − 2+ 3 ⎥ −bc1,0 L − bc0,0 L L ⎥ ⎦ 0

2 6z − L L2

(A.36)

The loading vector describing shrinkage effects pe.sh can be determined based on Eq. A.26c. If shrinkage does not vary along a member, fshN and fshM required to deﬁne f sh in Eq. A.26c are constant and for the AEMM are given by: Ee,k εsh,k dA = Ee,k Ac εsh,k and fshM = y Ee,k εsh,k dA = Ee,k Bc εsh,k fshN = Ac

Ac

The assumption of uniform shrinkage is usually acceptable for most practical applications.

Analytical formulations 403 The shrinkage loading vector pe.sh can then be calculated as: pe.sh = (A Ne )T fsh dz L

⎡

⎤

3 4z ⎢− + 2 ⎢ L L

⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ × ⎢ 4 − 8z 2 L⎢ ⎢ L L ⎢ 1 4z ⎢− + ⎢ L L2 ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎣ 0

⎤ ⎡ ⎥ ⎥ Ee,k Ac εsh,k ⎥ ⎥ ⎢ − ⎥ ⎢ 6 12z ⎥ ⎥ ⎥ ⎢ − 2 3 ⎥ ⎥ ⎢ 0 L L ⎥ ⎥ ⎢ ⎥ ⎢ 4 6z Ee,k Bc εsh,k ⎥ ⎥⎡ ⎥ ⎢ − ⎤ ⎥ ⎢ L L2 ⎥ L ⎥ ⎥ ⎢ ⎥ ⎣Ee,k Ac εsh,k ⎦ ⎥ ⎢ dz = ⎢ ⎥ ⎥ 0 0 ⎥ ⎥ ⎢ ⎥ Ee,k Bc εsh,k ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ Ee,k Ac εsh,k ⎥ 0 ⎥ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎥ ⎢ 6 12z ⎥ 0 ⎥ ⎢ − + ⎥ ⎦ ⎣ L2 L3 ⎥ Ee,k Bc εsh,k ⎦ − 2 6z 0

L

−

L2

(A.37)

L

A.4.2 Step-by-step method The 7 DOF ﬁnite element of the previous section is reconsidered here with the timedependent behaviour of the concrete described using the SSM. The change in the representation of the concrete time-dependent behaviour only affects the calculation of the loading vectors accounting for creep and shrinkage effects. In fact, the stiffness matrix and the vectors depicting member loads and shrinkage are always deﬁned using the cross-sectional properties relevant to the time step under consideration. In particular, with the SSM the concrete contributions are determined using Ec,k introduced in Eqs 4.25 and 4.26. Similarly to the AEMM, the loading vector describing creep effects pe.cr can be determined once the values of fcrN and fcrM included in f cr are determined. The expressions of these terms calculated using the SSM are deﬁned in Eqs A.15a and c. Also in this case, polynomials are utilized to represent the variation of the concrete axial force and moment along the element length measured at different time steps. For this purpose, the coefﬁcients included in these polynomials need to be recorded at each instant in time. Another possible approach would rely on the use of a numerical integration for the calculation of fcrN,k and fcrM,k . In this case, the concrete axial force and moment obtained at particular locations along each element (and required for the numerical integration) need to be stored. As the orders of the functions representing the concrete axial force and moment do not vary with time, the polynomials already identiﬁed for the AEMM in the previous example to describe the concrete instantaneous response are now adopted for each time instant. The concrete axial force and moment at time τi may be expressed as: Nc.i = ac0,i + ac1,i z

and Mc.i = bc0,i + bc1,i z

(A.38a,b)

and the coefﬁcients ac0,i , ac1,i , bc0,i , and bc1,i are determined as outlined in the following.

404 Analytical formulations Considering the constitutive relationship for concrete introduced in Eq. 4.25 (reproduced here for ease of reference): σc,i = Ec,i (εi − εsh ) +

k−1

Fe,k,n σc,n

n=0

the deﬁnitions of both axial force and moment resisted by the concrete component at any time τi can be expressed as: i−1 σc,i dA = Ec,i ui − yvi − Ec,i εsh,i + Fe,i,n σc,n d A Nc,i = Ac

Ac

n=0

= Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i + Mc,i =

Ac

yσc,i dA =

Ac

Fe,i,n Nc,n

(A.39a)

n=0

i−1 y Ec,i ui − yvi − Ec,i εsh,i + Fe,i,n σc,n d A

i−1

n=0

= Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n

(A.39b)

n=0

Considering Eqs A.27–A.30, the expressions for ui and vi required in Eqs A.39 are determined in terms of nodal displacements as:

3 4 1 4 8 4 ui = − uL,i + uM,i − uR,i + uL,i − 2 uM,i + 2 uR,i z (A.40a) L L L L2 L L

6 4 6 2 12 6 12 6 vi = − 2 vL,i − θL,i + 2 vR,i − θR,i + v + θ − v + θ L,i L,i R,i R,i z L L L L L3 L2 L3 L2 (A.40b) Substituting Eqs A.40 into Eq. A.39a produces the expression for Nc,i in terms of nodal displacements, shrinkage and previous loading history: Nc,i = Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i +

i−1

Fe,i,n Nc,n

n=0

3 4 1 4 8 4 = Ac Ec,i − uL,i + uM,i − uR,i + uL,i − 2 uM,i + 2 uR,i z L L L L2 L L

6 4 6 2 − Bc Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i L L L L

12 6 12 6 + v + θ − v + θ L,i L,i R,i R,i z L3 L2 L3 L2 − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n + ac1,n z

n=0

= ac0,i + ac1,i z

(A.41a)

Analytical formulations 405 where:

3 4 1 ac0,i = Ac Ec,i − uL,i + uM,i − uR,i L L L

6 4 6 2 − Bc Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i L L L L − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n

n=0

4 8 4 ac1,i = Ac Ec,i uL,i − 2 uM,i + 2 uR,i L2 L L

i−1 12 6 12 6 v + θ − v + θ + Fe,i,n ac1,n − Bc Ec,i L,i L,i R,i R,i L3 L2 L3 L2 n=0

Similarly, for Mc,i :

Mc,i = Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n = bc0,i + bc1,i z

(A.41b)

n=0

where:

3 4 1 bc0,i = Bc Ec,i − uL,i + uM,i − uR,i L L L

i−1 6 4 6 2 Fe,i,n bc0,n − Ic Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i − Bc Ec,i εsh,i + L L L L n=0

4 8 4 bc1,i = Bc Ec,i u − u + u L,i M,i R,i L2 L2 L2

i−1 12 6 12 6 + v + θ − v + θ Fe,i,n bc1,n − Ic Ec,i L,i L,i R,i R,i L3 L2 L3 L2 n=0

The expressions for fcrN,k and fcrM,k can then be re-written as:

fcrN,k =

k−1

Fe,k,i Nc,i =

i=0

fcrM,k =

k−1 i=0

k−1

Fe,k,i ac0,i + ac1,i z

i=0

Fe,k,i Mc,i =

k−1 i=0

Fe,k,i bc0,i + bc1,i z

406 Analytical formulations and the loading vector related to creep effects pe.cr is obtained from: pe.cr = (A Ne )T fcr dz L

⎡

⎤

⎢− 3 + 4z ⎥ 0 ⎢ L L2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎡ ⎤ ⎢ 12z ⎥ 6 L ⎢ 0 ⎥ − −ac0,i − ac1,i ⎢ L2 L3 ⎥ 6 ⎢ ⎥ ⎢ ⎥⎡ ⎢ ⎥ ⎤ ⎢ ⎥ −b c1,i ⎢ ⎥ 4 6z ⎥ ⎢ 0 ⎢ ⎥ − 2 ⎥ k−1 ⎢ ⎢ ⎢ ⎥ ⎥ L L b c0,i ⎥ ⎢ Fe,k,i ac0,i + ac1,i z ⎥ ⎢ k−1 ⎢ ⎥ ⎢ ⎥⎢ ⎥ ⎢ ⎥ ⎥ ⎢ i=0 Fe,k,i ⎢ − 2 Lac1,i ⎥ = ⎢ ⎥ dz = ⎢ 4 − 8z ⎥ 0 ⎢ ⎥ ⎢ ⎥ L ⎢ L L2 ⎥ ⎣k−1 ⎢5 3 ⎥ i=0 ⎢ ⎥ F b + b z⎦ ⎢ ⎥ La + a c0,i c1,i e,k,i ⎢ ⎥ ⎢ 6 c1,i c0,i ⎥ ⎢ 1 4z ⎥ i=0 ⎢ ⎥ 0 ⎢− + 2 ⎥ ⎣ ⎦ bc1,i ⎢ L L ⎥ ⎢ ⎥ ⎢ ⎥ −bc1,i L − bc0,i 12z 6 ⎢ 0 − 2+ 3 ⎥ ⎢ ⎥ L L ⎢ ⎥ ⎣ ⎦ 0

6z 2 − L L2

(A.42)

The loading vector related to shrinkage effects pe.sh is obtained from Eq. A.37, except that Ec,k replaces Ee,k .

A.5 Strong formulation (local balance condition) The strong form of the problem, consisting of the governing system of differential equations and corresponding boundary conditions, is obtained by integrating by parts the weak form presented in Eq. A.8, as follows: L L L Ni uˆ 0 − Ni uˆ dz − Mi vˆ 0 + Mi vˆ 0 − Mi vˆ dz =

L

L

L

pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL + SR vˆ R + NR uˆ R + MR θˆR

(A.43)

Enforcing horizontal and vertical equilibrium, the system of differential equations obtained from Eq. A.43 can then be expressed as: Ni + n = 0

and

Mi + p = 0

(A.44a,b)

From Eq. A.43, the corresponding boundary conditions to be applied at the left and right ends of the beam segment (i.e. at z = 0 and L) are: (NiL + NL ) uˆ L = 0; MiL + SL vˆ L = 0;

(NiR − NR ) uˆ R = 0 MiR − SR vˆ R = 0

(A.45a,b)

(MiL − ML ) θˆL = 0;

(MiR + MR ) θˆR = 0

(A.45e,f)

(A.45c,d)

Analytical formulations 407 The differential equations and their boundary conditions can also be deﬁned in terms of the independent displacements u and v by recalling the expressions for Ni and Mi of Eq. A.12: Ni = RA u − RB v + fcrN − fshN

(A.46a)

Mi = RB u − RI v + fcrM − fshM

(A.46b)

where the rigidities RA , RB and RI are deﬁned in Chapter 5 for different types of cross-sections. Substituting Eqs A.46 into Eqs A.44 and A.45 the differential equations can be re-written as: RA u − RB v + fcrN − fshN +n = 0

RB u − RI v

(A.47a)

+ fcrM − fshM +p = 0

(A.47b)

and the boundary conditions at the left (L) and right (R) ends of the member become: RA uL − RB vL + fcrNL − fshNL + NL uˆ L = 0 RA uR − RB vR + fcrNR − fshNR − NR uˆ R = 0 RB uL − RI vL + fcrML − fshML + SL vˆ L = 0 RB uR − RI vR + fcrMR − fshMR − SR vˆ R = 0 RB uL − RI vL + fcrML − fshML − ML θˆL = 0 RB uR − RI vR + fcrMR − fshMR + MR θˆR = 0

(A.48a) (A.48b) (A.48c) (A.48d) (A.48e) (A.48f)

The system of differential equations (Eqs A.47) is solved in the following, initially for the instantaneous material properties (i.e. no time effects) and then for the time analysis using the AEMM and the SSM. A.5.1 Instantaneous analysis Ignoring creep and shrinkage effects (i.e. fcrN = 0, fcrM = 0, fshN = 0 and fshM = 0), the general expressions for u and v which satisfy Eqs A.47 can be written as: v = α1 p

z4 z3 z2 + C1 + C2 + C3 z + C4 24 6 2

(A.49a)

u = α2 p

z3 z2 + (α3 C1 + α4 n) + C5 z + C6 6 2

(A.49b)

while the following coefﬁcients are been introduced to simplify the notation: α0 = R1 RA − R2B ;

α1 =

RA ; α0

α2 =

RB ; α0

α3 =

RB ; RA

and α4 =

−1 RA (A.50a–e)

408 Analytical formulations The constants of integration Cj (with j = 1, . . . , 6) can be determined based on the boundary conditions (Eqs A.48). In the following these analytical solutions have been used to derive the stiffness matrix and loading vector to be used in the stiffness method outlined in Chapter 9. A.5.1.1 Stiffness matrix Consider the unloaded ﬁxed ended beam shown in Fig. A.4a. The beam is modelled using a single 6 DOF stiffness element similar to that shown in Fig. 9.1 (i.e. three freedoms at each end node). The freedom numbering for the beam is shown in Fig. A.4b. The direct stiffness method is used here to derive the coefﬁcients of the stiffness matrix. The direct stiffness method is a procedure which enables the determination of the stiffness coefﬁcients by enforcing a unit displacement along one freedom while all other freedoms are restrained. The actual stiffness coefﬁcients are then equal to the reactions of the ﬁxed-ended beam required to keep the displaced conﬁguration. For example, enforcing a unit displacement along freedom 3 (i.e. rotation at the left support in Fig. A.4b), the reactions of the ﬁxed-ended beam correspond to the coefﬁcients included in the third column of the stiffness matrix. This approach is useful only when there is an analytical or numerical solution available to calculate the sought end reactions shown in Fig. A.4c. In the following, this will be carried out using the analytical solutions presented in Eqs A.49 combined with the boundary conditions of Eqs A.48. In order to calculate the coefﬁcients of the ﬁrst column of the stiffness matrix, a unit displacement is enforced along freedom 1 (Fig. A.4b), which corresponds to the axial displacement of the left node. For clarity, this deformation is shown in Fig. A.5. Considering that both member ends are fully restrained by the ﬁxed support conditions, the constants of integration included in the general solutions for u and v presented in Eqs A.49 can be determined by enforcing the following kinematic conditions:

6

3

z

1

4

2

L (a) Support conditions

5 (b) Numbering of the freedoms

ML

MR NR

NL SL

SR

z L (c) Freebody diagram

Figure A.4 Unloaded, ﬁxed-ended beam.

Analytical formulations 409 0

0

1

0

0

0

Figure A.5 A unit displacement enforced along freedom 1.

u (z = 0) = 1; u (z = L) = 0; and θ (z = L) = 0.

v (z = 0) = 0;

v (z = L) = 0;

θ (z = 0) = 0;

The calculated constants of integration can then be written as: C1 = 0;

C2 = 0;

C3 = 0;

C4 = 0;

1 C5 = − ; and C6 = 1. L

Adopting the static boundary conditions of Eqs A.48, the reactions of the ﬁxedended beam can be determined by solving the following equations for the unknown nodal actions (which represent the desired reactions): RA uL − RB vL + NL = 0;

RA uR − RB vR − NR = 0

RB uL − RI vL + SL = 0;

RB uR − RI vR − SR = 0

RB uL − RI vL − ML = 0;

RB uR − RI vR + MR = 0

where the expressions related to creep and shrinkage have been omitted as not relevant to the calculations of the stiffness coefﬁcients. The reactions required to maintain this deformed conﬁguration (Fig. A.5) can be collected in the following vector: ⎤ ⎡ ⎡ ⎤ RA /L NL ⎥ ⎢ ⎢ ⎥ ⎢ SL ⎥ ⎢ 0 ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ML ⎥ ⎢ RB /L ⎥ p1 = ⎢ ⎥=⎢ ⎥ ⎢ NR ⎥ ⎢−RA /L⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎣ SR ⎦ ⎣ 0 ⎦ −RB /L MR which deﬁnes the ﬁrst column of the stiffness matrix (identiﬁed by the subscript ‘1’). Considering a unit displacement along freedom 2 (Fig. A.6), the boundary conditions necessary to determine the constants of integration are: u (z = 0) = 0;

u (z = L) = 0;

v (z = 0) = 1;

v (z = L) = 0;

θ (z = 0) = 0;

and θ (z = L) = 0. and these produce the following expressions: C1 =

12 ; L3

C2 = −

6 ; L2

C3 = 0;

C4 = 1;

C5 = −

6 RB ; and C6 = 0. L 2 RA

410 Analytical formulations 0 0

0

0

0 1

Figure A.6 A unit displacement enforced along freedom 2.

Based on these constants of integration, the analytical solution for this displaced conﬁguration is described by a cubic function for the deﬂection v and a parabolic one for the axial displacement u, therefore providing consistent contributions to the strain ﬁeld from both v and u. The reactions, which form the second column of the stiffness matrix, are determined using the static boundary conditions of Eqs A.48 as: ⎡

⎤

0

⎥ ⎢ ⎢ 12 RI RA − R2B ⎥ ⎥ ⎡ ⎢ ⎤ ⎥ ⎢ L3 RA 0 NL ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ SL ⎥ ⎢ 6 RI RA − R2B ⎥ ⎢ 12/α1 L3 ⎥ ⎥ ⎢ ⎥ ⎢− ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ RA ⎥ ⎢ −6/α1 L2 ⎥ ⎢ M L ⎥ ⎢ L2 p2 = ⎢ ⎥=⎢ ⎥=⎢ ⎥ ⎥ ⎢ ⎥ ⎢ NR ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎣ SR ⎦ ⎢ 12 RI RA − R2B ⎥ ⎣−12/α1 L3 ⎦ ⎥ ⎢− ⎥ ⎢ L3 MR −6/α1 L2 RA ⎥ ⎢ ⎥ ⎢ ⎣ 6 RI RA − R2 ⎦ B − 2 RA L ⎡

⎤

Considering the remaining freedoms one at the time, the coefﬁcients of the whole stiffness matrix are determined: ⎡ ⎢ RA ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ ⎢ RB ⎢− ⎢ ke = ⎢ L ⎢ ⎢ RA ⎢− ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎣ R B L

⎤ 0

RB − L

RA − L

12 α1 L3

6 α1 L2

0

−

12 α 1 L3

6 α1 L2

R2 4 + B α1 L R A L

RB L

−

6 α 1 L2

0

RB L

RA L

0

0

12 α1 L3

−

12 α1 L 3

6 α1 L2

−

6 α1 L2

R2 2 − B α1 L R A L

−

RB L

0

−

6 α 1 L2

RB L

⎥ ⎥ ⎥ ⎥ ⎥ 6 ⎥ ⎥ α1 L 2 ⎥ ⎥ 2 RB ⎥ 2 ⎥ ⎥ − α1 L R A L ⎥ ⎥ ⎥ ⎥ RB ⎥ − ⎥ L ⎥ ⎥ ⎥ 6 ⎥ − ⎥ 2 α1 L ⎥ ⎥ 2 RB ⎦ 4 + α1 L R A L

(A.51)

Analytical formulations 411 A.5.1.2 Equivalent nodal actions for member loads Consider the ﬁxed-ended beam of the previous section subjected to constant member loads n and p (Fig. A.7). Eqs A.49 are used here to determine the equivalent nodal loads required to be used in the stiffness method of analysis. Note that this set of actions corresponds to the opposite of the reactions of the ﬁxed ended beam illustrated in Fig. A.7. As both member ends are fully restrained, the kinematic boundary conditions are: u (z = 0) = 0;

u (z = L) = 0;

v (z = 0) = 0;

v (z = L) = 0;

θ (z = 0) = 0;

and θ (z = L) = 0 and the expressions for the constants of integration are: L L2 α1 p; C3 = 0; C4 = 0; C1 = − α1 p; C2 = 2 12 3α1 α3 − 2α2 2 L C5 = L p − α4 n; and C6 = 0. 12 2 The reactions are obtained by solving the static boundary conditions of Eqs A.48 (ignoring time effects): RA uL − RB vL + NL = 0;

RB uL − RI vL + SL = 0;

RB uL − RI vL − ML = 0

RA uR − RB vR − NR = 0;

RB uR − RI vR − SR = 0;

RB uR − RI vR + MR = 0

and are given by: ⎤ ⎡ ⎡ ⎤ ⎡ ⎤ 0 NL.m −L/2 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎢ α3 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L2 /12⎥ ⎢Lα3 /2⎥ pF.m = ⎢ ⎥=⎢ ⎥ p+⎢ ⎥n ⎢ NR.m ⎥ ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ ⎣ α3 ⎦ L2 /12 MR.m Lα3 /2

(A.52)

where pF.m represents the reactions of the ﬁxed-ended beam subjected to constant longitudinal and transverse distributed loads, i.e. n and p. The equivalent nodal loads are equal and opposite to the reactions of pF.m . p

p MR

ML n

n

NR

NL SL

z

SR

z

L

L

(a) Loading and support conditions

(b) Free body diagram

Figure A.7 Fixed-ended beam subjected to constant member loads.

412 Analytical formulations A.5.1.3 Post-processing of the instantaneous solution From the instantaneous analysis, the axial force and moment resisted by the concrete at time τ0 are obtained from Eq. A.33. The deﬂection v0 and axial deformation u0 at any point z along a member are: z4 z3 z2 4,0 + C1,0 + C2,0 + C3,0 z + C 24 6 2 2 z3 6,0 1,0 + α4,0 n z + C 5,0 z + C u0 = α2,0 p + α3,0 C 6 2 v0 = α1,0 p

(A.53a) (A.53b)

where the constants αi,0 (i = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τ0 . Using the nodal displacements at each end of the member, the constants of integration are given by: 1,0 = − α1,0 L p + 6 θR,0 + θL,0 − 12 vR,0 − vL,0 C 2 L2 L3 2 2,0 = α1,0 L p − 2 θR,0 + 2θL,0 + 6 vR,0 − vL,0 C 2 12 L L C3,0 = θL,0 ; C4,0 = vL,0

5,0 = 3α1,0 α3,0 − 2α2,0 L2 p − α4,0 L n − 3α3,0 θR,0 + θL,0 C 12 2 L uR,0 − uL,0 6α3,0 − vL,0 − vR,0 + L L2 C6,0 = uL,0

(A.54a) (A.54b) (A.54c,d)

(A.54e) (A.54f)

The expressions for u0 and v0 can then be obtained by differentiating Eqs A.53: u0 = α2,0 p

z2 1,0 + α4,0 n z + C 5,0 + α3,0 C 2

(A.55a)

v0 = α1,0 p

z2 2,0 + C1,0 z + C 2

(A.55b)

The internal actions resisted by the concrete component can then be re-written as: Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0 z2 1,0 + α4,0 n z + C 5,0 = Ac Ec,0 α2,0 p + α3,0 C 2 z2 2,0 − Bc Ec,0 α1,0 p + C1,0 z + C 2 = ac0,0 + ac1,0 z + ac2,0 z2

(A.56)

Analytical formulations 413 where: 5,0 −Bc Ec,0 C 2,0 , ac0,0 = Ac Ec,0 C

1,0 +Ac Ec,0 α4,0 n−Bc Ec,0 C 1,0 ac1,0 = Ac Ec,0 α3,0 C (A.57a,b)

ac2,0 =

Ac Ec,0 α2,0 p−Bc Ec,0 α1,0 p 2

(A.57c)

and Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0 z2 = Bc Ec,0 α2,0 p + α3,0 C1,0 + α4,0 n z + C5,0 2 z2 2,0 − Ic Ec,0 α1,0 p + C1,0 z + C 2 = bc0,0 + bc1,0 z + bc2,0 z2

(A.58)

where: 5,0 −Ic Ec,0 C 2,0 ; bc0,0 = Bc Ec,0 C

1,0 +Bc Ec,0 α4,0 n−Ic Ec,0 C 1,0 bc1,0 = Bc Ec α3,0 C (A.59a,b)

bc2,0 =

Bc Ec,0 α2,0 p−Ic Ec,0 α1,0 p 2

(A.59c)

A.5.2 Age-adjusted effective modulus method (AEMM) The differential equations and boundary conditions to be used for the time analysis require the knowledge of the functions fcrN and fcrM in Eqs A.47 and A.48. Expressions for these terms to be used with the AEMM can be obtained substituting Eqs A.56 and A.58 into Eqs A.14: fcrN = Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z + ac2,0 z2 fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z + bc2,0 z2

(A.60a) (A.60b)

and their ﬁrst and second derivatives, included in the system of differential equations, become: fcrN = Fe,0 ac1,0 + 2ac2,0 z ; fcrN = 2ac2,0 Fe,0 ;

fcrM = Fe,0 bc1,0 + 2bc2,0 z

fcrM = 2bc2,0 Fe,0

(A.61a,b) (A.61c,d)

Shrinkage effects are included using the same approach adopted for the ﬁnite element formulation in Section A4.1 where both fshN and fshM (related to shrinkage) are

414 Analytical formulations assumed to remain constant along the member length and when used with the AEMM are: fshN =

Ac

Ee,k Ac εsh,k and fshM = Ee,k εsh,k dA =

Ac

y Ee,k εsh,k dA = Ee,k Bc εsh,k (A.62a,b)

It is now possible to solve the differential equations (Eqs A.47) as a function of the axial displacement and deﬂection at time τk by substituting Eqs A.60 and A.62 into Eqs A.47: z3 z2 uk = α2,k p + β2,k + α3,k C1,k + α4,k n + β3,k + C5,k z + C6,k 6 2 z4 z3 z2 + C1,k + C2,k + C3,k z + C4,k vk = α1,k p + β1,k 24 6 2

(A.63a) (A.63b)

where the constants αi,k (i = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τk and the constants βi,k (i = 1 to 3) are given by: β1,k =

2RA bc2,0 Fe,0 − 2RB ac2,0 Fe,0 α0,k

β2,k =

RB 2ac2,0 Fe,0 β1,k − RA RA

and β3,k = −

(A.64a) ac1,0 Fe,0 RA

(A.64b,c)

The equivalent nodal loads required to account for member loads, creep and shrinkage are determined in the following worked example. A.5.2.1 Equivalent nodal actions at time τk Consider the ﬁxed-ended beam of the previous sections (shown in Fig. A.7) subjected to constant member loads n and p, as well as creep and shrinkage effects. The equivalent nodal loads required in the stiffness method to simulate member loads, creep and shrinkage effects are here determined separately using the general solution in Eqs A.63. From the boundary conditions for the ﬁxed ended beam (i.e. uL,k = uR,k = vL,k = vR,k = θL,k = θR,k = 0), the following expressions for the constants of integration are determined: C1,k = −

C5,k =

α1,k p + β1,k L; 2

C2,k =

α1,k p + β1,k 2 L ; 12

C3,k = 0;

C4,k = 0 (A.65a–d)

3α1,k α3,k − 2α2,k 2 α4,k α3,k L2 L2 L L p− n+ β1,k − β − β ; C6,k = 0. 12 2 4 6 2,k 2 3,k (A.65e,f)

Analytical formulations 415 and the support reactions are then obtained solving (Eqs A.48): RA uL,k −RB vL,k +fcrNL −fshNL +NL = 0;

RA uR,k −RB vR,k +fcrNR −fshNR −NR = 0;

+fcrML −fshML +SL = 0; RB uL,k −RI vL,k

RB uR,k −RI vR,k +fcrMR −fshMR −SR = 0;

+fcrML −fshML −ML = 0; RB uL,k −RI vL,k

RB uR,k −RI vR,k +fcrMR −fshMR +MR = 0.

The results have been summarized below for each loading condition considered separately. The three sets of reactions pF.m , pF.sh and pF.cr are the opposite of the equivalent nodal loads required in the stiffness method to handle these loading conditions: ⎤ ⎡ ⎤ ⎡ ⎡ ⎤ ⎡ ⎤ 0 NL.m Ee,k Ac εsh,k −L/2 ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎢ ⎢ α3,k ⎥ 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L /12⎥ ⎢−Ee,k Bc εsh,k ⎥ ⎢Lα3,k /2⎥ pF.m = ⎢ ⎥=⎢ ⎥ ⎥ p+⎢ ⎥ n; pF.sh = ⎢ ⎥ ⎢ NR.m ⎥ ⎢ 0 ⎥ ⎢− ⎢ −L/2 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ Ee,k Ac εsh,k ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ 0 ⎦ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ ⎣ ⎣ −α3,k ⎦ 2 L /12 MR.m Lα3,k /2 Ee,k Bc εsh,k ⎡

ac2,0 L2 ac1,0 L + + ac0,0 − Fe,0 3 2

(A.66a,b)

⎤

⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 ⎢ ⎥ ac1,0 + ac2,0 L L ⎢ ⎥ − L − b + b α − F e,0 c0,0 c2,0 3,k ⎢ ⎥ 2 6 ⎢ ⎥ pF.cr = ⎢ ⎥ 2 ⎢ ⎥ a L L a c2,0 c1,0 ⎢ ⎥ Fe,0 + + ac0,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ − Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 ac1,0 + ac2,0 L 5L ⎦ ⎣ −Fe,0 − α3,k L + bc0,0 + bc1,0 L + bc2,0 2 6

(A.66c)

A.5.2.2 Post-processing of the solution at time τk The expressions for uk and vk to be used in the post-processing are given in Eqs A.63. Considering that both creep and shrinkage have been included in the analysis using equivalent nodal actions it is necessary to solve the governing system of differential equations at time τk (Eqs A.47) using the nodal displacements at that time as boundary conditions. The relevant constants of integration (for Eqs A.63) can be obtained using Eqs A.48 as: 1,k = − α1,k p+β1,k L+ 6 θR,k +θL,k − 12 vR,k −vL,k ; C 2 3 2 L L

3,k = θR,k C (A.67a,b)

416 Analytical formulations α 2,k = 1,k p+β1,k L2 − 2 θR,k +2θL,k + 6 vR,k −vL,k ; C 2 12 L L 5,k = C

6,k = uL,k . 4,k = vL,k ; C C

3α1,k α3,k −2α2,k 2 α4,k α3,k L2 L2 L L p− n+ β1,k − β2,k − β3,k 12 2 4 6 2 6α3,k uR,k −uL,k 3α3,k − θR,k +θL,k − 2 vL,k −vR,k + L L L

(A.67c–e)

(A.67f)

Based on these, the expressions for uk and vk which deﬁne the strain diagram at τk can be written as: z2 1,k + α4,k n + β3,k z + C 5,k uk = α2,k p + β2,k + α3,k C 2 z2 2,k 1,k z + C +C vk = α1,k p + β1,k 2

(A.68a) (A.68b)

For completeness, the expressions for the internal actions resisted by the concrete at τk can be determined as follows: Ee,k uk − Bc Ee,k vk − Ac Ee,k εsh,k + Fe,0 Nc,0 Nc.k = Ac z2 1,k + α4,k n + β3,k z + C 5,k = Ac Ee,k α2,k p + β2,k + α3,k C 2 z2 1,k z + C 2,k − Bc Ee,k α1,k p + β1,k +C 2 − Ac Ee,k εsh,k + Fe,0 ac0,0 + ac1,0 z + ac2,0 z2 = ac0,k + ac1,k z + ac2,k z2

(A.69a)

Mc.k = Bc Ee,k uk − Ic Ee,k vk − Bc Ee,k εsh,k + Fe,0 Mc,0 z2 = Bc Ee,k α2,k p + β2,k + α3,k C1,k + α4,k n + β3,k z + C5,k 2 z2 − Ic Ee,k α1,k p + β1,k + C1,k z + C2,k 2 − Bc Ee,k εsh,k + Fe,0 bc0,0 + bc1,0 z + bc2,0 z2 = bc0,k + bc1,k z + bc2,k z2

(A.69b)

where: 5,k − Bc 2,k − Ac Ee,k C Ee,k C Ee,k εsh,k + Fe,0 ac0,0 ac0,k = Ac 1,k + α4,k n + β3,k − Bc 1,k + ac1,k = Ac Ee,k α3,k C Ee,k C Fe,0 ac1,0

(A.70a) (A.70b)

Analytical formulations 417 α p + β α p + β 2,k 2,k 1,k 1,k Ee,k Ee,k (A.70c) − Bc + Fe,0 ac2,0 ac2,k = Ac 2 2 5,k − Ic 2,k − Bc bc0,k = Bc Ee,k C Ee,k C Ee,k εsh,k + Fe,0 bc0,0

(A.70d)

1,k + α4,k n + β3,k − Ic 1,k + bc1,k = Bc Ee,k α3,k C Ee,k C Fe,0 bc1,0

(A.70e)

Ee,k bc2,k = Bc

α2,k p + β2,k α1,k p + β1,k − Ic Ee,k + Fe,0 bc2,0 2 2

(A.70f)

A.5.3 Step-by-step method (SSM) The time-dependent response of a beam segment calculated using the SSM is obtained by solving the system of differential (Eqs A.47) and corresponding boundary conditions (Eqs A.48) at time τk using the following expressions for fcrN,k and fcrM,k (Eqs A.15):

fcrN,k =

k−1 i=0

fcrM,k =

k−1 i=0

Ac

Fe,k,i σc,i dA =

k−1

(A.71a)

i=0

Ac

Fe,k,i Nc,i

yFe,k,i σc,i dA =

k−1

Fe,k,i Mc,i

(A.71b)

i=0

where the coefﬁcient Fe,k,i are deﬁned in Eq. 4.25, while the internal actions resisted by the concrete at times τi (Nc,i and Mc,i ) are given in Eqs A.39. It is assumed that the internal actions (i.e. Nc,n and Mc,n ) resisted by the concrete in previous time steps τn (with n = 0, . . . , i − 1) are known and available. Based on the fact that the format of the polynomials or functions describing the concrete internal actions do not vary with time, it is possible to derive the basic expressions for Nc,n and Mc,n from the results of the instantaneous analysis. This was already carried out when considering the AEMM leading to the use of parabolic expressions for both Nc,n and Mc,n (Eqs A.56 and A.58) assuming both member loads n and p to remain constant. These can be written for the generic time step τn required in Eqs A.39 as: Nc,n = ac0,n + ac1,n z + ac2,n z2

(A.72a)

Mc,n = bc0,n + bc1,n z + bc2,n z2

(A.72b)

where the coefﬁcients ac0,n and bc0,n are assumed to be known for n < i. The coefﬁcients describing the internal actions at time τi are obtained in the following by substituting ui and vi determined at time τi into Eqs A.39. For this purpose, the expressions for ui and vi are obtained by solving the system of differential equations of Eqs A.47 enforcing the kinematic boundary conditions consistent with the nodal displacements calculated from the stiffness method at time τi .

418 Analytical formulations The functions fcrN,i and fcrM,i are obtained substituting Nc,n and Mc,n into Eqs A.71:

fcrN,i =

i−1 n=0 Ac

Fe,i,n σc,n dA =

i−1

Fe,i,n Nc,n =

n=0

i−1

Fe,i,n ac0,n + ac1,n z + ac2,n z2

n=0

(A.73a) fcrM,i =

i−1 n=0 Ac

yFe,i,n σc,n dA =

i−1

Fe,i,n Mc,n =

n=0

i−1

Fe,i,n bc0,n + bc1,n z + bc2,n z2

n=0

(A.73b) and their ﬁrst and second derivatives become: fcrN,i =

i−1

Fe,i,n ac1,n + 2ac2,n z ;

fcrM,i =

n=0 fcrN,i

=

i−1

i−1

Fe,i,n bc1,n + 2bc2,n z

(A.74a)

n=0

2ac2,n Fe,i,n ;

n=0

fcrM,i

=

i−1

2bc2,n Fe,i,n

(A.74b)

n=0

Under the assumptions of constant shrinkage exhibited along the member length, the expressions for fshN,i and fshM,i are: fshN,i =

Ac

Ec,i εsh,i dA = Ec,i Ac εsh,i and fshM,i =

Ac

yEc,i εsh,i dA = Ec,i Bc εsh,i (A.75a,b)

Substituting Eqs A.73 to A.75 into Eqs A.47 the system of differential equations can be written at time τi as: RA ui − RB vi +

i−1

Fe,i,n ac1,n + 2ac2,n z + n = 0

(A.76a)

Fe,i,n bc1,n + 2bc2,n z + p = 0

(A.76b)

n=0

RB ui − RI vi +

i−1 n=0

This can be solved for ui and vi giving: z3 2 1,i + α4,i n + β3,i z + C 6,i 5,i z + C + α3,i C ui = α2,i p + β2,i 6 2 3 2 z4 1,i z + C 2,i z + C 3,i z + C 4,i +C vi = α1,i p + β1,i 24 6 2

(A.77a) (A.77b)

Analytical formulations 419 where the constants αj,i (j = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τi and the constants βj,i (j = 1 to 3) are given by: 2RA β1,i =

i−1 0

bc2,n Fe,i,n − 2RB

n=0

i−1 0

ac2,n Fe,i,n

n=0

(A.78a)

α0,i

RB β2,i = β1,i − RA

2

i−1 0

i−1 0

ac2,n Fe,i,n

n=0

RA

and β3,i = −

ac1,n Fe,i,n

n=0

(A.78b,c)

RA

The constants of integration required to deﬁne the displacements along the member lengths based on the solution at time τi (i.e. ui and vi ) are obtained by enforcing the boundary conditions at that time and are given by: 1,i = − α1,i p+β1,i L+ 6 θR,i +θL,i − 12 vR,i −vL,i ; C 3,i = θL,i C 2 3 2 L L 4,i = vL,i ; 2,i = α1,i p+β1,i L2 − 2 θR,i +2θL,i + 6 vR,i −vL,i ; C C 2 12 L L 2 2 5,i = 3α1,i α3,i −2α2,i L2 p− α4,i n+ α3,i L β1,i − L β2,i − L β3,i C 12 2 4 6 2 6α3,i uR,i −uL,i 3α3,i − 2 vL,i −vR,i + − vR,i +vL,i L L L

(A.79a,b) 6,i = uL,i C (A.79c–e)

(A.79f)

For the time instant τi the strain diagram can be deﬁned by substituting the constants of integration of Eqs A.79 into Eqs A.77 and differentiating: z2 5,i 1,i + α4,i n + β3,i z + C + α3,i C ui = α2,i p + β2,i 2 z2 2,i 1,i z + C +C vi = α1,i p + β1,i 2

(A.80a) (A.80b)

Substituting Eqs A.80 with the calculated constants of integrations (Eqs A.79) into Eqs A.39 gives: Nc.i = Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i +

i−1

Fe,i,n Nc,n

n=0

z2 1,i + α4,i n + β3,i z + C 5,i = Ac Ec,i α2,i p + β2,i + α3,i C 2 z2 − Bc Ec,i α1,i p + β1,i + C1,i z + C2,i 2

420 Analytical formulations − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n + ac1,n z + ac2,n z2

n=0

= ac0,i + ac1,i z + ac2,i z2

(A.81)

where: 5,i − Bc Ec,i C 2,i − Ac Ec,i εsh,i + ac0,i = Ac Ec,i C

i−1

Fe,i,n ac0,n

(A.82a)

n=0 i−1 1,i + α4,i n + β3,i − Bc Ec,i C 1,i + ac1,i = Ac Ec,i α3,i C Fe,i,n ac1,n

(A.82b)

n=0

α2,i p + β2,i α1,i p + β1,i Fe,i,n ac2,n − Bc Ec,i + 2 2 i−1

ac2,i = Ac Ec,i

(A.82c)

n=0

Similarly, for Mc,i : Mc,i = Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n

n=0

z2 5,i 1,i + α4,i n + β3,i z + C = Bc Ec,i α2,i p + β2,i + α3,i C 2 z2 2,i 1,i z + C − Ic Ec,i α1,i p + β1,i +C 2 − Bc Ec,i εsh,i +

i−1

Fe,i,n bc0,n + bc1,n z + bc2,n z2

n=0

= bc0,i + bc1,i z + bc2,i z2

(A.83)

where: 5,i − Ic Ec,i C 2,i − Bc Ec,i εsh,i + bc0,i = Bc Ec,i C

i−1

Fe,i,n bc0,n

(A.84a)

n=0 i−1 1,i + α4,i n + β3,i − Ic Ec,i C 1,i + bc1,i = Bc Ec,i α3,i C Fe,i,n bc1,n

(A.84b)

n=0

α2,i p + β2,i α1,i p + β1,i − Ic Ec,i + Fe,i,n bc2,n 2 2 i−1

bc2,i = Bc Ec,i

(A.84c)

n=0

It is now possible to address the solution of the problem at time τk which will be used in the following example to determine the equivalent nodal actions to be used with

Analytical formulations 421 the SSM. This is now possible as the loading history of the concrete can be calculated and recorded for each previous time step τi (i < k) based on Eqs A.81 and A.83. Also, these can be used to deﬁne the expressions for fcrN.k and fcrM.k (Eqs A.14) required in the solution based on the creep effects due to stress increments at all previous time instants: fcrN,k =

k−1

Fe,k,i Nc,i =

i=0

fcrM,k =

k−1

Fe,k,i ac0,i + ac1,i z + ac2,i z2

(A.85a)

Fe,k,i bc0,i + bc1,i z + bc2,i z2

(A.85b)

i=0

k−1

Fe,k,i Mc,i =

i=0

k−1 i=0

with corresponding derivatives: fcrN,k =

k−1

Fe,k,i ac1,i + 2ac2,i z

and fcrM =

i=0

k−1

Fe,k,i bc1,i + 2bc2,i z

i=0

(A.86a,b) fcrN =

k−1

2ac2,i Fe,k,i

i=0

and fcrM =

k−1

2bc2,i Fe,k,i

(A.86c,d)

i=0

Using the notation adopted for the SSM, the shrinkage effects are: fshN,k =

Ac

Ec,k εsh,k dA = Ec,k Ac εsh,k and fshM,k =

Ac

yEc,k εsh,k dA = Ec,k Bc εsh,k (A.87a,b)

Substituting Eqs A.85 and A.87 into Eqs A.47 produces the governing system of differential equations: RA uk − RB vk +

k−1

Fe,k,i ac1,i + 2ac2,i z + n = 0

(A.88a)

Fe,k,i bc1,i + 2bc2,i z + p = 0

(A.88b)

i=0

RB uk − RI vk +

k−1 i=0

whose general solution can be expressed as: z3 z2 + α3,k C1,k + α4,k n + β3,k + C5,k z + C6,k uk = α2,k p + β2,k 6 2 z4 z3 z2 + C1,k + C2,k + C3,k z + C4,k vk = α1,k p + β1,k 24 6 2

(A.89a) (A.89b)

422 Analytical formulations where the constants αj,k (j = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τk and the constants βj,i (j = 1 to 3) are given by:

2RA

k−1 0 i=0

β1,k =

k−1 0

bc2,i Fe,k,i − 2RB

i=0

ac2,i Fe,k,i

RB β2,k = β − RA 1,k

;

α0,k

2

k−1 0 i=0

ac2,i Fe,k,i RA (A.90a,b)

k−1 0

β3,k = −

i=0

ac1,i Fe,k,i (A.90c)

RA

A.5.3.1 Equivalent nodal actions at time τk Based on the ﬁxed-ended beam of the previous section (Fig. A.7), the expressions for the equivalent nodal loads required to account for member loads n and p, creep effects and shrinkage effects in the stiffness method are here determined using the SSM. The constants of integration to deﬁne the expressions for the axial displacement uk and deﬂection vk at time τk are identical to those obtained for the AEMM (and given in Eqs A.65) as the material properties are included in the coefﬁcients αj,k and βj,k . The end reactions at the ﬁxed supports are then obtained applying the static boundary conditions of Eqs A.48: + fcrNL,k − fshNL,k + NL = 0 RA uL,k − RB vL,k + fcrNR,k − fshNR,k − NR = 0 RA uR,k − RB vR,k + fcrML,k − fshML,k + SL = 0 RB uL,k − RI vL,k + fcrMR,k − fshMR,k − SR = 0 RB uR,k − RI vR,k + fcrML,k − fshML,k − ML = 0 RB uL,k − RI vL,k + fcrMR,k − fshMR,k + MR = 0 RB uR,k − RI vR,k

The vectors pF.m , pF.sh and pF.cr can be deﬁned as: ⎡

NL.m

⎤

⎡

0

⎤

⎡

−L/2

⎤

⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ α3,k ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L2 /12⎥ ⎥=⎢ ⎥ p + ⎢Lα3,k /2⎥ n; pF.m = ⎢ ⎢ −L/2 ⎥ ⎢N ⎥ ⎢ 0 ⎥ ⎥ ⎢ ⎥ ⎢ R.m ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎣ −α3,k ⎦ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ MR.m

L2 /12

Lα3,k /2

⎡

Ec,k Ac εsh,k

⎤

⎥ ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎢−Ec,k Bc εsh,k ⎥ ⎥ pF.sh = ⎢ ⎢−E A ε ⎥ (A.91a,b) ⎢ c,k c sh,k ⎥ ⎥ ⎢ ⎦ ⎣ 0 Ec,k Bc εsh,k

⎡

Analytical formulations 423 ⎤

k−1 0 ac2,i L2 ac1,i L ⎢ ⎥ F + + ac0,i − e,k,i ⎢ ⎥ 3 2 i=0 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ k−1 0 ⎢ ⎥ Fe,k,i α3,k ac1,i + Lα3,k ac2,i − bc1,i − bc2,i L ⎢ ⎥ ⎢ ⎥ i=0 ⎢ ⎥ ⎢ ⎥ 2 k−1 0 ac1,i + ac2,i L L ⎢ ⎥ − Fe,k,i − α3,k L − bc0,i + bc2,i ⎢ ⎥ ⎢ ⎥ 2 6 i=0 ⎥ pF.cr = ⎢ ⎢ ⎥ 2 k−1 ⎢ ⎥ 0 a L a L c2,i c1,i ⎢ ⎥ Fe,k,i + + ac0,i ⎢ ⎥ 3 2 i=0 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ k−1 0 ⎢ ⎥ − Fe,k,i α3,k ac1,i + Lα3,k ac2,i − bc1,i − bc2,i L ⎢ ⎥ ⎢ ⎥ i=0 ⎢ ⎥ ⎢ k−1 ⎥ 2 ac1,i + ac2,i L 5L ⎦ ⎣ 0 − Fe,k,i − α3,k L + bc0,i + bc1,i L + bc2,i 2 6 i=0

(A.91c)

As expected these loading vectors are very similar to those already calculated using the AEMM. For example, Eqs A.91 are identical to Eqs A.66 with the only difference relying on the way the instantaneous concrete modulus is determined with the AEMM and SSM. The equivalent nodal actions for use in the stiffness method are equal and opposite to pF.m , pF.cr and pF.sh . A.5.3.2 Post-processing of the solution at time τi In the case of the SSM the expressions for the axial displacement ui and deﬂection vi required for the post-processing of the solution at any time instant have already been derived in Eqs A.77. For a time τi , the constants of integration deﬁning ui and vi are obtained using Eqs A.79. The expressions for ui and vi deﬁning the strain diagram at τi are given in Eqs A.80. For completeness, the internal actions resisted by the concrete component can be determined using Eqs A.81 and A.83.

A.6 References 1. Bathe, K.-J. (2006). Finite Element Procedures. Prentice Hall, Pearson Education, New Jersey. 2. Reddy, J.N. (2004). An Introduction to the Finite Element Method. Third edition, McGraw-Hill, New York. 3. Gupta, A.K. and Ma, P.S. (1977). Error in eccentric beam formulation. International Journal for Numerical Methods in Engineering, 11, 1473–1483. 4. Crisﬁeld, M.A. (1991). The eccentricity issue in the design if plate and shell elements. Communications in applied Numerical Methods, 7, 47–56. 5. Ranzi, G. and Zona, A. (2007). A composite beam model including the shear deformability of the steel component. Engineering Structures, 29, 3026–3041.

Index

ACI 318-08 57–9, 62–4 Afﬁnity assumption 130 Age-adjusted: effective modulus for concrete 121; effective modulus method (AEMM) 119–28, 151–64, 244–56; modular ratio 122; transformed section 156 Aging 8, 22: effect of 8 Aging coefﬁcient 119, 122–5; equations for 123–4; graphs for 124 Aspect ratio, Ly /Lx 327 AS3600-2009 57–9, 60–2; models for creep and shrinkage 26–31 Axial deformation 49–51 Axial rigidity 141 Basic creep 5 Biaxial bending 224–59 Bridge decks, thermal gradients 342 Column 101, 335–40 Column strip 330 Composite cross-sections: concrete-concrete 189–222; steel-concrete 180–9 Compressive strength of concrete 24 Constitutive relationships for concrete 22, 100, 106, 122, 127, 130 Continuity stresses 341, 349 Continuous structures see Indeterminate structures Cover-controlled cracks 261 Cracking: cover-controlled cracks 261; crack control 75–96; direct tension cracking 91–6; simpliﬁed code approaches for ﬂexural cracking 76–83; tension chord model for ﬂexural cracking 83–91; cracked cross-sections: effective cracked sections 57; effect of creep 16; effect of shrinkage 20; short-term analysis 54–6, 265–79; time-dependent analysis: AEMM 279–88; step-by-step method 288–92; cracked members: deﬂection of 49–75, 301–4

crack spacing: direct tension 95; ﬂexural 83–7 crack width determination: direct tension 91–6; ﬂexural 76–91 crack width limits 44, 45; direct tension cracks 75, 91–6; ﬂexural cracks 75–91; primary cracks 53, 83, 260–1; recommended maximum design crack widths 45; secondary cracks 261; shrinkage cracks 91–6; tension stiffening 37, 52–4, 261–2 Creep coefﬁcient 8–9, 26–9 Creep function 8–9 Creep of concrete: basic creep 5; basic ﬂow 7; creep coefﬁcient 8–9, 26–9; creep function 8–9; creep problems 3; delayed elastic strain 7; drying creep 5; drying ﬂow 7; effect of: age at loading 8; relative humidity 6; size and shape of member 6; strength of concrete 6; stress level 6; temperature 6; effect on: axially loaded members 15; behaviour of structures 14–17; composite sections 187; fully-cracked reinforced concrete section 16; indeterminate prestressed members 320–2; moment–curvature relationship 264; slender columns 335–6; uncracked sections 16; ﬂow 7; inﬂuencing factors 5–6; integral-type creep law 13; irrecoverable creep 7; linear creep 6; mechanisms 5–6; non-linear creep 6; rapid initial ﬂow 7; recoverable creep 7; speciﬁc creep 9; tensile creep 14 Creep of prestressing steel 34–6 Crossing beam analogy 326 Cross-sectional analysis: cracked sections: short-term at time τ0 54–6, 265–79; time-dependent (AEMM) at τk 279–88; time-dependent (SSM) at τj 288–92; uncracked sections: short-term at time τ0 138–51, 189–92, 226–44; time-dependent (AEMM) at τk 119–28, 151–64, 192–4,

Index 425 244–56; time-dependent (SSM) at τj 105–19, 164–80, 200–3, 256–9 Cross-sectional rigidities: short-term at time τ0 140–2, 227–9, 269–70, 289; time-dependent (AEMM) at τk 154–5, 245–6, 280; time-dependent (SSM) at τj 167, 257, 291 Curvature: due to axial force and biaxial bending 224–5; due to axial force and uniaxial bending 137–8; due to creep 16; effect of non-prestressed steel on 297–301; integration of 50; due to shrinkage 20; due to temperature 341 Deﬂection: calculation from curvature at ends and at mid-span 49–52; calculation (recommended procedure) 69–75; at column mid-length 335–6; control using non-prestressed reinforcement 297–301; of cracked statically determinate beams 301–4; by double integration of curvature 50; in edge-supported slabs 326; in ﬂat slabs 330; incremental deﬂection 42–3; limits 41–4; long-term multiplication factor 58–9; problems 41–2; total deﬂection 42–3; of uncracked statically determinate beams 294–6 Delayed elasticity 7 Density of concrete 26 Depth to the neutral axis of a cracked section 54–5, 266–71 Designing for serviceability 38–44: crack width limits 44–5; deﬂection limits 41–4; design actions 39–41; design objectives and criteria 38–9; incremental deﬂection 42–3; total deﬂection 42–3; vibration control 44 Dischinger’s equation of state 130 Drying creep 5 Edge-supported two-way slab 326–30 Effective modular ratio 102 Effective modulus method (EMM) 100–5 Effective modulus of concrete 9, 100 Effective second moment of area (effective moment of inertia) 57 Eigenstresses: due to non-linear shrinkage 19; due to non-linear temperature 340 Elastic modulus of concrete 25–6 Elastic strain 2–3 Environmental loads 40 Equivalent nodal actions 411, 422 Euler-Bernoulli beam assumptions 261, 355, 391 Eurocode 2, 64–9, 77–9

Finite element analysis: for cracked members 387–90; formulation 396–406; for uncracked members 376–83 Flat slabs 330–5 Flexibility coefﬁcients 307 Flexibility matrix 307 Force method 306 Frame element 355 Indeterminate structures 305–24 Instantaneous concrete strain 2–3 Integral-type creep law 13 Irrecoverable creep 7 Kinematic model 392 Limit states design 39 Linear creep 6 Loads on structures: environmental loads 40; expected loads 40; load combinations for serviceability 40; speciﬁed (or characteristic) loads 40 Load versus deﬂection response 52–3 Long-term deﬂection multiplication factor 58 Loss of prestress 163, 301 Mechanisms of creep 5–6 Member loads 354 Middle strip 330 Modular ratio 54 Modular ratio theory 52, 54–6 Moment–curvature relationships 262–4 Moment redistribution 14, 20, 306, 320, 322 Non-linear creep 6 Non-linear strain distributions 19, 341 Non-linear temperature distributions 341–2 Non-prestressed steel 32–3 Parallel creep curve assumption 129 Post-processing solutions: instantaneous 412–13; time analysis 413–23 Post-tensioned beam 294 Prestressing steel 33–6 Pretensioned plank 323 Primary cracks 53, 83, 261 Primary structure 306 Principle of superposition 9–14, 105–19 Rate of creep method (RCM) 128–33 Redundant forces 305–16 Reinforcement see Steel reinforcement Relaxation of prestressing steel 34–6 Relaxation problems 3 Restrained shrinkage 20, 92

426

Index

Rigidities: short-term at time τ0 140–2, 227–9, 269–70, 289; time-dependent (AEMM) at τk 154–5, 245–6, 280; time-dependent (SSM) at τj 167, 257, 291 Secondary cracks 261 Secondary actions 320, 335, 341 Second moment of area: cracked section 53, 56; effective 53, 57; uncracked section 53 Serviceability limit states 39 Settlement of supports 316 Shrinkage of concrete: autogenous shrinkage 17; chemical shrinkage 17 drying shrinkage 17, 30; effect of: aggregate type, 18; relative humidity 18; size and shape of member 18; water–cement ratio 18; effect on: behaviour of structures 18–22; moment–curvature relationship 264; eigenstresses 19; endogenous shrinkage 17, 29–30; induced tension 20, 57; inﬂuencing factors 18; method for predicting 29–31; non-linear distribution 19; plastic shrinkage 17; prediction of 29–31; self-equilibrating stresses 19, 340–1; shrinkage-induced curvature 20; thermal shrinkage 17 Sign convention xiv–xix Slab stiffness factor 327 Slabs see Two-way slabs Slender columns 335–40; iterative analysis 336; primary and secondary moments 335 Slope 50 Solar radiation 341 Span-to-depth ratio 44–9 Speciﬁc creep 9 Statically determinate members 293–4 Statically indeterminate members 305–24; determination of redundants 306–8; effect of support settlement 316–17; effects of creep 320–2 Steel reinforcement 31–6; conventional or non-prestressed reinforcement 32–3; prestressing steel: creep coefﬁcient 35–6; relaxation 34–6; relaxation reduction due to concrete creep and shrinkage, 35–6; wire, strand and bar 33–6

Step-by-step method (SSM) 105–9, 256–9 Stiffness matrix 352, 410 Stiffness method 351–4 Strain components 2–3 Strain magnitudes 4–5 Superposition equation 11, 106–7 Support settlement 316–20 Temperature effects: coefﬁcients of thermal expansion 342; continuity stresses 349; cross-sectional analysis 341–4; eigenstresses 340; on magnitude of creep 6; non-linear distribution 341–2; redundant forces 347; self-equilibrating, 340 Tensile creep 14 Tensile strength of concrete 24–5 Tension chord model 83–91 Tension stiffening 37, 41, 52–4, 57, 70, 77, 84 Thermal effects see Temperature effects Time analyses: basic concepts 22; of cracked cross-sections 279–80, 290–1; ﬁnite element method 376–83, 387–90; of indeterminate members 305–8; stiffness method 361–3, 368; of uncracked cross-sections: axial loading 105–10, 114–17, 119–22, 127, 128–30; biaxial bending 244–7, 256–9; composite concrete-concrete sections 192–4; composite steel-concrete sections 180–2; reinforced and prestressed sections in uniaxial bending 151–7, 164–9 Time discretisation 105–6 Transformed section 143, 270 Trost-Bazant Method 119 Two-way slabs: deﬂection components 331; deﬂection models 325–6; deﬂection problems 324; edge-supported slabs 326–7; ﬁnite element models 325–6; ﬂat slabs 330–1; maximum span-to-depth ratio 46–7; wide beam method 330 Vibration control 44 Wide beam method 330

View more...
Serviceability failures of concrete structures involving excessive cracking or deﬂection are relatively common, even in structures that comply with code requirements. This is often as a result of a failure to adequately account for the time-dependent deformations of concrete in the design of the structure. Design for serviceability is complicated by the non-linear and inelastic behaviour of concrete at service loads. The serviceability provisions embodied in codes of practice are relatively crude and, in some situations, may be unreliable and often do not adequately model the in-service behaviour of structures. In particular, they fail to realistically account for the effects of creep and shrinkage of the concrete. Providing detailed information, this book assists engineers to rationally predict the time-varying deformation of concrete structures under typical in-service conditions. It gives analytical methods to help anticipate time-dependent cracking, the gradual change in tension stiffening with time, creep-induced deformations and the load independent strains caused by shrinkage and temperature changes. Calculation procedures are illustrated with many worked examples. A vital guide for practising engineers and advanced students of structural engineering on the design of concrete structures for serviceability, providing a penetrating insight into the time-dependent behaviour of reinforced and prestressed concrete structures. Raymond Ian Gilbert is Professor of Civil Engineering at the University of New South Wales and currently holds an Australian Research Council Australian Professorial Fellowships. He has over 35 years experience in structural design and is a specialist in the analysis and design of reinforced and prestressed concrete structures. Gianluca Ranzi is a Senior Lecturer of Structural Engineering at the University of Sydney, specialising in the analysis and design of concrete and composite steel-concrete structures.

Time-Dependent Behaviour of Concrete Structures

Raymond Ian Gilbert and Gianluca Ranzi

First published 2011 by Spon Press 2 Park Square, Milton Park, Abingdon, Oxon OX14 4RN Simultaneously published in the USA and Canada by Spon Press 270 Madison Avenue, New York, NY 10016 USA

This edition published in the Taylor & Francis e-Library, 2010. To purchase your own copy of this or any of Taylor & Francis or Routledge’s collection of thousands of eBooks please go to www.eBookstore.tandf.co.uk. Spon Press is an imprint of the Taylor & Francis Group, an informa business © 2011 Raymond Ian Gilbert and Gianluca Ranzi All rights reserved. No part of this book may be reprinted or reproduced or utilised in any form or by any electronic, mechanical, or other means, now known or hereafter invented, including photocopying and recording, or in any information storage or retrieval system, without permission in writing from the publishers. This publication presents material of a broad scope and applicability. Despite stringent efforts by all concerned in the publishing process, some typographical or editorial errors may occur, and readers are encouraged to bring these to our attention where they represent errors of substance. The publisher and author disclaim any liability, in whole or in part, arising from information contained in this publication. The reader is urged to consult with an appropriate licensed professional prior to taking any action or making any interpretation that is within the realm of a licensed professional practice. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library Library of Congress Cataloging-in-Publication Data Gilbert, R. I., 1950– Time-dependent behaviour of concrete structures / Raymond Ian Gilbert and Gianluca Ranzi. p. cm. Includes bibliographical references and index. 1. Concrete–Deterioration. 2. Service life (Engineering) 3. Concrete structures. I. Ranzi, Gianluca, 1972– II. Title. TA440.G449 2010 2010007786 624.1 834–dc22

ISBN 0-203-87939-2 Master e-book ISBN ISBN13: 978-0-415-49384-0 (hbk) ISBN13: 978-0-203-87939-9 (ebk)

Contents

Preface Acknowledgements Notation and sign convention

xi xiii xiv

1 Time-dependent deformation

1

1.1

1.2

1.3

1.4 1.5

Background 1 1.1.1 Concrete strain components 2 1.1.2 Typical concrete strain magnitudes 4 Creep of concrete 5 1.2.1 Creep mechanisms and inﬂuencing factors 5 1.2.2 Creep components 7 1.2.3 Effects of ageing 8 1.2.4 The creep coefﬁcient, ϕ (t, τ ), and the creep function, J (t, τ ) 8 1.2.5 The principle of superposition 9 1.2.6 Tensile creep 14 1.2.7 The effects of creep on structural behaviour 14 Shrinkage of concrete 17 1.3.1 Types of shrinkage 17 1.3.2 Factors affecting shrinkage 18 1.3.3 The effects of shrinkage on structural behaviour 18 Time analysis – the basic problem 22 References 22

2 Material properties 2.1

Concrete 24 2.1.1 Introductory remarks 24 2.1.2 Compressive and tensile strength 24 2.1.3 Elastic modulus 25 2.1.4 Creep coefﬁcient 26 2.1.5 Shrinkage strain 29

24

vi Contents 2.2

Steel reinforcement 31 2.2.1 General 31 2.2.2 Conventional, non-prestressed reinforcement 32 2.2.3 Prestressing steel 33 2.3 References 36

3 Design for serviceability – deﬂection and crack control 3.1 3.2 3.3 3.4

Introduction 37 Design objectives and criteria 38 Design actions 39 Design criteria for serviceability 41 3.4.1 Deﬂection limits 41 3.4.2 Crack width limits 44 3.5 Maximum span-to-depth ratio – minimum thickness 44 Example 3.1 48 3.6 Deﬂection control by simpliﬁed calculation 49 3.6.1 Calculation of deformation 49 3.6.2 Load versus deﬂection response of a reinforced concrete member 52 3.6.3 Modular ratio theory 54 3.6.4 AS 3600-2009 and ACI 318-08 57 3.6.4.1 3.6.4.2

3.6.5

Instantaneous deﬂection 57 Time-dependent deﬂection 58

Example 3.2 59 Eurocode 2 64 3.6.5.1 3.6.5.2

Instantaneous curvature 64 Time-dependent curvature 65

Example 3.3 65 3.6.6 Recommended simpliﬁed approach 69 3.6.6.1 3.6.6.2 3.6.6.3

3.7

Instantaneous deﬂection 69 Time-dependent creep-induced curvature 70 Time-dependent shrinkage-induced curvature 71

Example 3.4 72 Crack control 75 3.7.1 General 75 3.7.2 Simpliﬁed code-oriented approaches for ﬂexural crack control 76 3.7.2.1 3.7.2.2 3.7.2.3 3.7.2.4 3.7.2.5

3.7.3

Gergely and Lutz 76 Frosch 77 Eurocode 2 – 1992 77 Eurocode 2 – 2004 77 ACI 318-08 79

Example 3.5 79 Tension chord model for ﬂexural cracking in reinforced concrete 83

37

Contents

vii

Example 3.6 87 Example 3.7 89 3.7.4 Model for direct tension cracking in restrained reinforced concrete 91 Example 3.8 95 3.8 References 96

4 Uncracked sections – axial loading

99

4.1 4.2

Preamble 99 The effective modulus method 100 4.2.1 Formulation 100 4.2.2 Example application (EMM) 101 Example 4.1 103 4.3 The principle of superposition – step-by-step method (SSM) 105 4.3.1 Formulation 105 4.3.2 Example application (SSM) – Approach 1 108 4.3.2.1 4.3.2.2

At ﬁrst loading (t = τ0 ) 108 At the end of the j-th time step (i.e. t = τj ) 108

Example 4.2 110 Example application (SSM) – Approach 2 114 Example 4.3 117 The age-adjusted effective modulus method (AEMM) 119 4.4.1 Formulation 119 4.4.2 Example application (AEMM) – Approach 1 121 4.4.3 Determination of the ageing coefﬁcient 122 Example 4.4 125 4.4.4 Example application (AEMM) – Approach 2 127 Example 4.5 128 The rate of creep method (RCM) 128 4.5.1 Formulation 128 4.5.2 Discussion 130 4.5.3 Example application (RCM) 130 Example 4.6 132 Comparison of methods of analysis 133 References 136 4.3.3

4.4

4.5

4.6 4.7

5 Uncracked sections – axial force and uniaxial bending 5.1 5.2 5.3

Introductory remarks 137 Overview of cross-sectional analysis 137 Short-term analysis of reinforced or prestressed concrete cross-sections 138 Example 5.1 143 Example 5.2 147

137

viii Contents 5.4

5.5

5.6

5.7

5.8

Long-term analysis of reinforced or prestressed concrete cross-sections using the age-adjusted effective modulus method (AEMM) 151 Example 5.3 157 Example 5.4 161 Long-term analysis of reinforced and prestressed cross-sections using the step-by-step procedure 164 Example 5.5 169 Example 5.6 174 Composite steel-concrete cross-sections 180 Example 5.7 182 Example 5.8 187 Composite concrete-concrete cross-sections 189 5.7.1 Short-term analysis 190 5.7.2 Time analysis – AEMM 192 Example 5.9 194 5.7.3 Time analysis – SSM 200 Example 5.10 203 References 223

6 Uncracked sections – axial force and biaxial bending

224

6.1 6.2

Introduction 224 Short-term analysis 226 Example 6.1 233 Example 6.2 236 Example 6.3 240 6.3 Long-term analysis using the age-adjusted effective modulus method (AEMM) 244 Example 6.4 248 Example 6.5 251 6.4 Long-term analysis using the step-by-step method 256

7 Cracked sections 7.1 7.2

Introductory remarks 260 Short-term analysis 265 7.2.1 Axial force and uniaxial bending 266 Example 7.1 271 Example 7.2 275 7.2.2 Axial force and biaxial bending 278 7.3 Time-dependent analysis (AEMM) 279 7.3.1 Axial force and uniaxial bending 279 Example 7.3 280 Example 7.4 285 7.3.2 Axial force and biaxial bending 288

260

Contents 7.4

ix

Short- and long-term analysis using the step-by-step method 288 7.4.1 Axial force and uniaxial bending 288 7.4.1.1 7.4.1.2

Instantaneous analysis 288 Time analysis 290

7.4.2 Axial force and biaxial bending 291 7.5 References 292

8 Members and structures 8.1 8.2

8.3

8.4

8.5

8.6

8.7 8.8

Introductory remarks 293 Deﬂection of statically determinate beams 293 8.2.1 Deﬂection and axial shortening of uncracked beams 293 Example 8.1 294 8.2.2 Control of deﬂection using non-prestressed reinforcement 297 8.2.3 Deﬂection and axial shortening of cracked beams 301 Example 8.2 302 Statically indeterminate beams and slabs 305 8.3.1 Discussion 305 8.3.2 Determination of redundants 306 Example 8.3 308 Example 8.4 310 8.3.3 Effects of deformation or settlement at the supports 316 Example 8.5 317 8.3.4 Further effects of creep in prestressed construction 320 Example 8.6 323 Two-way slab systems 324 8.4.1 Discussion 324 8.4.2 Slab deﬂection models 325 8.4.3 Two-way edge-supported slabs 326 Example 8.7 327 8.4.4 Flat slabs 330 Example 8.8 331 Slender reinforced concrete columns 335 8.5.1 Discussion 335 8.5.2 An iterative method of analysis 336 Example 8.9 337 Temperature effects 340 8.6.1 Introduction 340 8.6.2 Temperature distributions 341 8.6.3 Temperature analysis of cross-sections 341 Example 8.10 344 8.6.4 Temperature effects in members and structures 347 Example 8.11 347 Concluding remarks 349 References 349

293

x Contents

9 Stiffness method and ﬁnite-element modelling 9.1 9.2 9.3 9.4 9.5 9.6

9.7

9.8

351

Introduction 351 Overview of the stiffness method 351 Member loads 354 Example 9.1 356 Time analysis using AEMM 361 Example 9.2 363 Time analysis using SSM 368 Example 9.3 368 Time analysis using the ﬁnite-element method 376 9.6.1 Load vector to account for time effects using the AEMM 380 9.6.2 Load vector to account for time effects using the SSM 381 9.6.3 Remarks on the consistency requirements for ﬁnite elements 381 Example 9.4 383 Analysis of cracked members 387 9.7.1 Approach 1 387 9.7.2 Approach 2 389 References 389

Appendix A Analytical formulations – Euler-Bernoulli beam model

391

A.1 A.2 A.3 A.4

Introduction 391 Kinematic model 392 Weak formulation (global balance condition) 393 Finite element formulation 396 A.4.1 Age-adjusted effective modulus method 397 A.4.2 Step-by-step method 403 A.5 Strong formulation (local balance condition) 406 A.5.1 Instantaneous analysis 407 A.5.1.1 A.5.1.2 A.5.1.3

A.5.2

Age-adjusted effective modulus method (AEMM) 413 A.5.2.1 A.5.2.2

A.5.3

Index

Equivalent nodal actions at time τk 414 Post-processing of the solution at time τk 415

Step-by-step method (SSM) 417 A.5.3.1 A.5.3.2

A.6

Stiffness matrix 408 Equivalent nodal actions for member loads 411 Post-processing of the instantaneous solution 412

Equivalent nodal actions at time τk 422 Post-processing of the solution at time τi 423

References 423

424

Preface

In the design of concrete structures, the two main design objectives are strength and serviceability. A structure must be strong enough and sufﬁciently ductile to resist, without collapsing, the overloads and environmental extremes that may be imposed on it. It must also perform satisfactorily under the day-to-day service loads without deforming, cracking or vibrating excessively. This book is concerned with the serviceability of concrete structures, in particular the prediction of instantaneous and time-dependent deformation under in-service conditions. The factors that most affect structural behaviour at the serviceability limit states are considered in considerable depth, including cracking of the tensile concrete, tension stiffening, and the timedependent deformations caused by creep and shrinkage of the concrete. The prediction of the ﬁnal deformation of a concrete structure, and the ﬁnal extent and width of cracks, are perhaps the most uncertain and least well-understood aspect of structural design. The long-term behaviour of the structure depends primarily on the deformational characteristics of the concrete, including its creep and shrinkage characteristics, and these are highly variable, depending not only on the mix proportions and types of cement and aggregates, but also on the local environment and the load history. In most undergraduate civil and structural engineering courses, the effects of concrete creep and shrinkage on structural behaviour are treated superﬁcially, with only the simpliﬁed code-oriented procedures for deﬂection and crack control being presented. The same is true of most books on the design of concrete structures. Failure to recognise and quantify the non-linear effects of cracking, creep and shrinkage is a common cause of serviceability failure. Creep and shrinkage of concrete and their effects on structural behaviour have been actively researched for over 100 years. Much has been written on the subject and many outstanding contributions have been made. However, much of the information and many of the analytical procedures that have been developed are not, in general, known or used by the profession. Structural designers often rely on the simpliﬁed procedures in codes of practice to estimate service load behaviour, and this often oversimpliﬁes the problem and can be unreliable. This book is an attempt to provide practising engineers and post-graduate students with a practical and useful treatment of the serviceability analysis of concrete structures. For this purpose, most sections included in each chapter are self-contained so that they can be read independently from the rest of the book. The analytical techniques are illustrated by numerous worked examples. In Chapter 1, an introductory discussion of concrete creep and shrinkage and their effects on the deformation of concrete structures is presented, while typical

xii Preface material properties and a simple procedure for estimating the creep and shrinkage characteristics of concrete are provided in Chapter 2. No attempt has been made to provide a detailed description of the mechanisms of creep and shrinkage or the factors affecting them. The material properties and material constitutive relationships are only of interest insofar as they affect the methods of structural analysis. Chapter 3 contains a qualitative discussion of structural behaviour at service loads and the simpliﬁed methods for the control of deﬂection and cracking contained in several of the major codes of practice are presented and critically reviewed, including ACI318-08, Eurocode 2 and the Australian Standard AS3600-2009. Alternative and more reliable procedures for deﬂection calculation and crack control are also provided. Chapters 4–7 deal with the time-dependent analysis of cross-sections, exploring various procedures for predicting the gradual change of strain and curvature with time and the gradual redistribution of stress between the concrete and the bonded steel reinforcement. Chapter 4 examines cross-sections loaded in axial compression. Chapter 5 considers a wide range of uncracked reinforced, prestressed and composite cross-sections carrying axial force and uniaxial bending. Chapter 6 deals with uncracked cross-sections subject to combined axial force and biaxial bending. Cracked cross-sections subjected to axial force and bending are analysed in Chapter 7. In Chapter 8, a range of different structural applications are considered, drawing on the cross-sectional analyses in Chapters 4–7 and the treatment of tension stiffening and cracking in Chapter 3. The techniques described and illustrated may be extended readily to include a wide range of additional structural applications. The procedures are not daunting and require little more than an elementary background in mechanics and structural analysis. Chapter 9 illustrates how the time-dependent effects of creep and shrinkage can be readily included in the computer analysis of structures using the stiffness and the ﬁniteelement methods. These have been described and applied considering the common Euler–Bernoulli beam model as a case study, but the approach is general and can be extended to more complex models. The analytical formulations required to implement the computer analysis of Chapter 9 are presented in Appendix A. It is hoped that this book will provide structural engineers not only with useful analytical tools to predict and control in-service performance, but also with a clearer picture of the interaction between concrete and reinforcement at service loads and a better understanding of why concrete structures behave as they do. Raymond Ian Gilbert and Gianluca Ranzi Sydney, 2010.

Acknowledgements

The authors acknowledge the support given by their respective institutions and by the Australian Research Council through its Discovery and Linkage schemes and the award of an ARC Australian Professorial Fellowship for the period 2005 to 2010 to the ﬁrst author. Thanks are also extended to Associate Professor Graziano Leoni and Dr Andrew Kilpatrick for their comments on the drafts of each chapter and to Associate Professor Rob Wheen for providing the cover photograph of the Anzac Bridge during construction.

Notation and sign convention

All symbols are deﬁned in the text where they ﬁrst appear. The more frequently used symbols and those that appear throughout the book are listed below. It is assumed that tension is positive and compression is negative, and positive bending about a horizontal axis causes tension in the bottom ﬁbres of a cross-section. A, B, I

A c , B c , Ic Ae , Be , I e Ass , Bss , Iss Act As(i) , Ap(i) Ast , Asc b, bw b∗ C C(t, τ0 ) c D0 , D j , D k D d db ds(i) , dp(i) dn (=kd) do dref

area, ﬁrst moment of area, and second moment of area, respectively, calculated about the reference axis of the cross-section properties A, B and I of the concrete part of the cross-section properties A, B and I of the age-adjusted transformed cross-section properties A, B and I of the structural steel part of a composite cross-section area of tensile concrete in the tension chord (Eq. 3.45) areas of the ith layer of non-prestressed and prestressed steel, respectively areas of tensile and compressive steel on a reinforced section, respectively ﬂange width and web width of a T-section width of cross-section at the level of the centroid of the tensile reinforcement speciﬁc creep (also Celsius) speciﬁc creep at time t produced by a sustained unit stress ﬁrst applied at τ0 concrete cover to reinforcement matrices of cross-sectional rigidities at τ0 , τj and τk , respectively overall depth of a cross-section effective depth of the tensile reinforcement bar diameter depths to the i-th layer of the non-prestressed and prestressed steel, respectively depth to the neutral axis on a fully-cracked cross-section depth from extreme compressive ﬁbre to the centroid of the outermost layer of tensile reinforcement depth of reference axis below the top ﬁbre of the cross-section

Notation and sign convention xv Ec , Es , Ep , Ess Ec,j Ee , Ee Ee,j,i e eAB eL f cr,j , f cr,k f set,j , f set,k f p,init f sh,j , f sh,k F F 0 , Fj , F k Fe,j,i Fe,0 fc , ft fc fcm , fcmi fct fct,f fji fp fst fy G, g Icr , Iuncr Ief Ig i, j, k h J J(t, τ0 ) Jj,i K

elastic moduli of concrete, non-prestressed steel, prestressed steel, and structural steel, respectively elastic modulus of concrete at time τj effective modulus of concrete (Eq. 4.3) and age-adjusted effective modulus of concrete (Eq. 4.35), respectively effective modulus of concrete at time τj due to a stress ﬁrst applied at τi eccentricity; base of the natural logarithm axial deformation of member AB axial shortening of a column of length, L vectors of actions at times τj and τk , respectively, accounting for creep during previous time periods vectors of corrected internal actions to be used at times τj and τk , respectively, when a new element is added to a cross-section vector of initial prestressing forces vectors of actions at times τj and τk , respectively, accounting for shrinkage during previous time periods ﬂexibility matrix matrices relating strain to internal actions on cross-section at τ0 , τj and τk , respectively creep factor at time τj for a stress applied at τi (Eq. 4.26b) age-adjusted creep factor (Eq. 4.46) strength of concrete in compression and in tension, respectively characteristic strength of concrete in compression mean concrete cylinder strength and mean concrete in-situ strength, respectively uniaxial tensile strength of concrete characteristic ﬂexural tensile strength of concrete (modulus of rupture) a ﬂexibility coefﬁcient (the displacement at release j due to a unit value of the ith redundant force) breaking strength of the prestressing steel steel stress on a cracked section corresponding to a crack width of w∗ yield stress of the non-prestressed steel dead load (kN) and dead load per unit area (kPa), respectively second moments of area of the fully-cracked and uncracked transformed cross-section about the centroidal axis, respectively effective second moment of area after cracking second moment of area of gross cross-section about centroidal axis integers slab thickness creep function creep function at time t for concrete ﬁrst loaded at τ0 (Eq. 1.10) creep function at time τj due to a stress ﬁrst applied at τi structural stiffness matrix

xvi Notation and sign convention kd kcs ke k1 , k2 , k3 , k4 , k5 L, Lx , Ly ln ef M Mcr Ms∗ Mu Mxe , Mye mc mp , ms Nc,0 , Ns,0 , Np,0 Nc,k , Ns,k , Np,k Ncr Ne , Me Ni,0 , Mi,0 Ni,k , Mi,k Nsus , Msus n ne , ne ne,j,i P P Pcr Pp,init p Q, q R RA,0 , RB,0 , RI,0 RA,k , RB,k , RI,k Rb RP RR re,k ri,k S

depth to neutral axis from extreme compressive ﬁbre long-term to short-term deﬂection multiplication factor element stiffness matrix factors describing the magnitude and rate of development of creep and shrinkage span of a beam or length of a column orthogonal span lengths for two-way slabs the natural logarithm the effective span (the lesser of the centre-to-centre distance between the supports and the clear span plus the member depth) moment cracking moment design in-service moment at the critical cross-section ultimate ﬂexural strength applied moments about the x- and y-axes, respectively number of layers of concrete in a discretised cross-section number of layers of tendons and non-prestressed reinforcement on a cross-section internal forces resisted by concrete, reinforcement and tendons at time τ0 , respectively internal forces resisted by concrete, reinforcement and tendons at time τk , respectively restraining force after direct tension cracking external axial force and moment applied to a cross-section internal axial force and moment on a cross-section at time τ0 internal axial force and moment on a cross-section at time τk sustained axial force and moment applied to a cross-section modular ratio (Es /Ec ) effective and age-adjusted effective modular ratios (Es /Ee , Es / Ee ), respectively effective modular ratio (Es /Ee,j,i ) vector of nodal loads for whole structure axial load; also prestressing force cracking load initial prestressing force prior to transfer vector of nodal loads for element live load (kN) and live load per unit area (kPa), respectively design relaxation force in the prestressing steel cross-sectional rigidities at time τ0 cross-sectional rigidities at time τk basic relaxation vector of reactions caused by loads on the primary structure vector of redundant forces vector of external actions at time τk vector of internal actions at time τk ﬁrst moment of area of the steel reinforcement about the centroid of the section

Notation and sign convention xvii s sb smax so s∗ T t th U u ue v vcx vmy vsus W w w∗ ws x y yn,0 ys , y p Z z α α1 , α2 , α3 β ε, κ δ δB ε εtop , εbtm ε˙ εcr εcr (t, τ0 ) ∗ εcr εe εr εr0 , εrk εp

spacing between cracks in the tensile zone maximum bar spacing maximum crack spacing immediately after loading distance over which the stresses vary on each side of a direct tension crack ﬁnal maximum crack spacing temperature; also tensile force time hypothetical thickness vector of nodal displacements for whole structure vector of nodal displacements for element portion of section perimeter exposed to the atmosphere deﬂection deﬂection of a column strip in the x-direction deﬂection of a middle strip in the y-direction deﬂection due to sustained loading wind load crack width; also uniformly distributed load maximum design crack width uniformly distributed sustained service load reference axis transverse distance from the reference axis in the plane of the section distance of neutral axis from x-axis on a cracked section at time τ0 y-coordinates of steel reinforcement and tendons, respectively section modulus direction of member axis coefﬁcient of thermal expansion; also a parameter to account for cracking and reinforcement on the change in deformation due to creep (Eqs 3.32) coefﬁcients associated with creep and shrinkage models (Sections 2.1.4 and 2.1.5) tension stiffening coefﬁcient to account for duration of loading an increment or a change change in strain and curvature with time, respectively lateral displacement of a slender column settlement at support B strain strains at the top and bottom ﬁbres of a cross-section, respectively rate of change of strain with time (dε/dt) creep strain creep strain at time t due to a stress ﬁrst applied at τ0 ﬁnal creep strain at time inﬁnity instantaneous (elastic) strain strain at reference axis strain at reference axis at time τ0 and at time τk , respectively strain in the prestressing steel

xviii Notation and sign convention εp,init εp.rel,k εs εsh εshd εshe ∗ εsh εT θ θM θNA κ κcr , κuncr κ0 , κk κsh κx , κy λr R λ 1 , λ2 , λ3 με ρ, ρ ρw , ρcw σ σc , σs σc,0 , σs,0 σc,k , σs,k σcs σp,init σ˙ σp(i) , σs(i) σst1 σtop τ τ0 τb τd τi τk ϕ ϕ(t, τ0 ) ϕbasic ϕj,i

initial strain in the prestressing steel before transfer relaxation strain in the prestressing steel at time τk strain in the steel reinforcement shrinkage strain drying shrinkage strain endogenous (chemical plus thermal) shrinkage strain ﬁnal shrinkage strain at time inﬁnity temperature component of strain slope angle between moment axis and the x-axis angle between the neutral axis and the x-axis curvature curvatures on fully-cracked and uncracked cross-section, respectively curvatures at time τ0 and at time τk , respectively curvature induced by shrinkage curvature with respect to the x-axis and y-axis, respectively reduced relaxation in the prestressing steel accounting for creep and shrinkage factors affecting bond stress microstrain (10−6 ) tensile reinforcement ratio Ast /bd (or Ast /Ac ) and compressive reinforcement ratio, Asc /bd, respectively or; also, density web reinforcement ratio for the tensile steel ((Ast + Apt )/bw d) and compressive steel (Asc /bw d), respectively the sum of stress concrete and steel stresses, respectively initial concrete and steel stresses, respectively, at ﬁrst loading, τ0 ﬁnal concrete and steel stresses, respectively, at time τk shrinkage-induced tensile stress in the concrete initial stress in the prestressing steel prior to transfer rate of change of concrete stress with time, dσ /dt stresses in the i-th layer of prestressed and non-prestressed steel, respectively tensile steel stress at a crack concrete stress at top ﬁbre of cross-section time instant; also shear stress age at ﬁrst loading bond shear stress age at the commencement of drying i-th time instant ﬁnal time instant at the end of the period of the time analysis creep coefﬁcient creep coefﬁcient at time t for concrete loaded at τ0 basic creep coefﬁcient creep coefﬁcient at time τj due to a stress ﬁrst applied at τi

Notation and sign convention xix ϕ˙ ϕp ϕ∗ χ χ(t, τ0 ) χ∗ ψ1 , ψ2 ζ ∞

rate of change of the creep coefﬁcient with time, dϕ/dt creep coefﬁcient for the prestressing steel ﬁnal creep coefﬁcient at time inﬁnity ageing coefﬁcient ageing coefﬁcient at time t for concrete ﬁrst loaded at τ0 ﬁnal ageing coefﬁcient at time inﬁnity short- and long-term serviceability load factors distribution factor to account for tension stiffening (Eq. 3.24) inﬁnity

1

Time-dependent deformation

1.1 Background When a concrete specimen is subjected to load, its response is both immediate and timedependent. Under sustained load, the deformation of a specimen gradually increases with time and eventually may be many times greater than its initial value. In order to satisfy the design objective of serviceability in a structural design, accurate and reliable predictions of the instantaneous and time-dependent deformation of the concrete structure are required. If the temperature and stress remain constant, the gradual development of strain with time is caused by creep and shrinkage. Creep strain is produced by sustained stress, while shrinkage strain is independent of stress. These inelastic and timedependent strains cause increases in deformation and curvature, losses of prestress and redistribution of stresses and internal actions. Creep and shrinkage are often responsible for excessive deﬂection at service loads. Creep frequently causes excessive camber and/or shortening in prestressed members. In addition, restraint to shrinkage may cause time-dependent cracking that could lead to serviceability or durability failures. To accurately and efﬁciently predict these effects, the following two basic prerequisites are necessary: (i) reliable data for the creep and shrinkage characteristics of the particular concrete mix; and (ii) analytical and/or numerical procedures for the inclusion of these time effects in the analysis and design of the structure. A number of sources are available from which to obtain information on the properties of concrete (see Sections 2.1.2–2.1.5). However, a comparison of the data obtained from these sources indicates signiﬁcant differences. Laboratory tests may be undertaken to determine time-dependent material properties but this is often not a practical alternative. Designers seldom have the time or the inclination for longterm tests and then often cannot be sure that the concrete that has been tested in the laboratory is the same as that which will later be used in the structure. Even if testing is undertaken, the variability in the measured deformational properties of concrete is usually large. Coefﬁcients of variation of 20 per cent or more can be expected. To best

2 Time-dependent deformation account for the variability of material properties in structural design, probabilistic methods are required. However, existing design methods are usually deterministic and the inexact nature of the results of such procedures must be kept in mind. A number of analytical and numerical techniques are available for serviceability analysis and the design of reinforced and prestressed concrete structures. These range from simpliﬁed approaches for deﬂection and crack control contained in codes of practice, such as those presented and evaluated in Chapter 3, to the more reﬁned methods contained in Chapters 4–9. Each level of reﬁnement has its own set of simplifying assumptions and each has its advantages and disadvantages. Some are more suited to particular situations than others. Throughout the book, many worked examples are provided and a wide range of structural applications and situations are considered. The worked examples are also self-contained and may be read by practitioners who are more interested in using the ﬁnal equations rather than following their detailed derivations. However, for most applications, the mathematics associated with each analysis is quite straightforward and there are obvious advantages in understanding the development of the procedures. Methods of analysis that include the effects of creep and shrinkage in concrete structures are important in the design for serviceability. But perhaps even more importantly, such analyses can provide a clear picture of the interaction between concrete and steel and an otherwise unavailable insight into the mechanism of structural behaviour. A study of time effects can provide the structural designer with a far better feel for the task and a clearer understanding of why concrete structures behave as they do. 1.1.1 Concrete strain components At any time t, the total concrete strain ε(t) in an uncracked, uniaxially-loaded specimen consists of a number of components that include the instantaneous strain εe (t), creep strain εcr (t), shrinkage strain εsh (t) and temperature strain ε T (t). Although not strictly correct, it is usual to assume that all four components are independent and may be calculated separately and combined to obtain the total strain. When calculating the inservice behaviour of a concrete structure at constant temperature, it is usual to express the concrete strain at a point as the sum of the instantaneous, creep and shrinkage components: ε(t) = εe (t) + εcr (t) + εsh (t)

(1.1)

The strain components in a drying specimen held at constant temperature and subjected to a constant sustained compressive stress σc0 ﬁrst applied at time τ 0 are illustrated in Fig. 1.1. Immediately after the concrete sets or at the end of moist curing (t = τd in Fig. 1.1), shrinkage strains begin to develop and continue to increase at a decreasing rate. On the application of stress, a sudden jump in the strain diagram (instantaneous or elastic strain) is followed by an additional gradual increase in strain due to creep. The prediction of the time-dependent behaviour of a concrete member requires the accurate prediction of each of these strain components at critical locations. This requires knowledge of the stress history, in addition to accurate data for the

Time-dependent deformation 3

Total strain ecr(t) – creep ee(t) − instantaneous

esh(t) − shrinkage

0 td

t0

Time, t

t0

Time, t

Stress sc0

0

Figure 1.1 Concrete strain components under sustained load.

material properties. The stress history depends on both the applied load and the boundary conditions of the member. It has been common practice in previous studies of the deformation of concrete to distinguish between creep problems and relaxation problems. Creep problems are those in which the gradual increase in strain under a sustained stress is calculated. Relaxation problems are those in which the total strain is held constant with time and the gradual change in stress is calculated. Creep and relaxation problems differ only in their boundary conditions. Both involve the estimation of the individual strain components in Eq. 1.1. Relaxation problems have the additional constraint that the sum of the change of each strain component within any time interval is zero, that is, εe (t) + εcr (t) + εsh (t) = 0. When the total strain is held constant, the change of stress with time (relaxation) is simply the result of the gradual development of creep and shrinkage and the consequent equal and opposite change in the instantaneous strain. If creep and shrinkage increase with time, then the instantaneous strain εe (t) must decrease. There is little to be gained from separate studies of creep and relaxation type problems. In fact, in reinforced concrete structures, it is uncommon to ﬁnd situations which fall neatly into the categories of either creep or relaxation problems. Concrete is almost never free to deform without some form of restraint. Reinforcement provides internal restraint to creep and shrinkage, while real support conditions often provide signiﬁcant external restraint. On the other hand, a member is rarely restrained so completely that no deformation of the concrete is possible. Real problems often involve elements of both creep and relaxation, and fall between these two extremes. For the time analysis of concrete structures, attention should be focused squarely on the problem of establishing suitable constitutive relationships for concrete that can be used

4 Time-dependent deformation in the analysis of practical problems for the determination of the strain components of Eq. 1.1 at any point in the structure. 1.1.2 Typical concrete strain magnitudes It is important from the outset to ﬁrmly establish the signiﬁcance of each of the concrete strain components and their order of magnitude in typical in-service situations. Consider a point in a concrete specimen subjected to a constant, sustained compressive stress σ c0 applied at time τ0 and equal to 40 per cent of the characteristic compressive strength of concrete, i.e. σc0 = 0.4 fc . In properly designed concrete structures, concrete stresses rarely exceed this level under typical service loads. The instantaneous strain that occurs immediately upon application of the stress may be considered to be elastic at low stress levels, and therefore: εe (t) =

σc0 Ec (τ0 )

(1.2)

Information on the time-varying nature of the elastic modulus for concrete, Ec (t), is given in Section 2.1.3. However, for comparison between the order of magnitude of each of the strain components in Eq. 1.1, the elastic modulus may be taken as constant with time and approximately equal to 1000 fc . In this case, therefore, the elastic strain is approximated by: εe ≈

−0.4 fc = −0.0004 = −400 με 1000 fc

where the negative sign indicates that the applied stress and elastic strain are compressive. Under normal conditions, the ﬁnal creep strain at time inﬁnity εcr (∞) (denoted here ∗ ) that is produced by a constant sustained stress of this magnitude is usually as εcr between 1.5 and 4.0 times the initial elastic strain. The higher end of this range is for low-strength concrete loaded at early ages and at a low relative humidity. A typical ﬁnal creep strain for structural concrete subjected to constant stress of this level is 2.5 εe and, for this case, ∗ ≈ 2.5 εe = −1000με εcr ∗ ) depends on The ﬁnal shrinkage strain at time inﬁnity εsh (∞) (denoted here as εsh the concrete composition, the environment and the size and shape of the specimen. For concrete elements in building structures, a typical value is: ∗ ≈ −600 με εsh

The thermal strain produced by a change in temperature T = T − T0 is calculated from: T εT =

α dT T0

(1.3)

Time-dependent deformation 5 where T0 is the initial temperature and α is the coefﬁcient of thermal expansion that is approximately 10 × 10−6 /◦ C (but actually depends on temperature and moisture content). For a 20◦ C change in temperature, the change in thermal strain is approximately α T = 200 με. If the specimen under consideration is held at constant temperature, the total concrete strain at time inﬁnity (which may be considered as several years after loading) is: ∗ ∗ ε∗ = εe + εcr + εsh ≈ −400 − 1000 − 600 = −2000 με

(1.4)

Thus the magnitude of the ﬁnal strain is about ﬁve times the magnitude of the instantaneous elastic strain. It must be emphasised that the magnitudes of the creep and shrinkage considered here are typical and not extreme values. Therefore, when calculating the deformation of concrete structures, time effects must be included in a rational and systematic way. Elastic analyses that ignore the effects of creep and shrinkage may grossly underestimate ﬁnal deformations and, in the design of concrete structures for serviceability, are of little value.

1.2 Creep of concrete 1.2.1 Creep mechanisms and inﬂuencing factors When concrete is subjected to a sustained stress, creep strain develops gradually with time as shown in Fig. 1.1. Creep increases with time at a decreasing rate. In the period immediately after initial loading, creep develops rapidly, but the rate of increase slows appreciably with time. Creep is generally thought to approach a limiting value as the time after ﬁrst loading approaches inﬁnity. About 50 per cent of the ﬁnal creep develops in the ﬁrst 2–3 months and about 90 per cent after 2–3 years. After several years under load, the rate of change of creep with time is very small. Throughout this book, creep and shrinkage are treated as separate and independent phenomena. In reality, this is not the case. Creep is signiﬁcantly greater when accompanied by shrinkage. In a loaded specimen that is in hygral equilibrium with the ambient medium (i.e. no drying), the time-dependent deformation caused by stress is known as basic creep. The additional creep that occurs in a drying specimen is sensibly known as drying creep. Creep is usually calculated as the difference between the total time-dependent deformation of a loaded specimen and the shrinkage of a similar unloaded specimen. Creep is treated here as the time-dependent deformation in excess of shrinkage. Creep of concrete originates in the hardened cement paste that consists of a solid cement gel containing numerous capillary pores. The cement gel is made up of colloidal sheets of calcium silicate hydrates separated by spaces containing absorbed water. Creep is thought to be caused by several different and complex mechanisms not yet fully understood (Refs 1–7). Neville et al. (Ref. 4) identiﬁed the following mechanisms for creep: (i) sliding of the colloidal sheets in the cement gel between the layers of absorbed water – viscous ﬂow;

6 Time-dependent deformation (ii) expulsion and decomposition of the interlayer water within the cement gel – seepage; (iii) elastic deformation of the aggregate and the gel crystals as viscous ﬂow and seepage occur within the cement gel – delayed elasticity; (iv) local fracture within the cement gel involving the breakdown (and formation) of physical bonds – microcracking; (v) mechanical deformation theory; and (vi) plastic ﬂow. Recent research relates the creep response to the packaging density distributions of calcium-silicate-hydrates (Ref. 7). At high stress levels, additional deformation occurs due to the breakdown of the bond between the cement paste and aggregate particles. Further references on creep mechanisms can be found in Refs 1 and 8. Many factors inﬂuence the magnitude and rate of development of creep. Some are properties of the concrete mix, while others depend on the environmental and loading conditions. In general, the capacity of the concrete to creep decreases as the concrete strength increases. For a particular stress level, creep in higher-strength concrete is less than that in lower-strength concrete. An increase in either the aggregate content or the maximum aggregate size reduces creep, as does the use of a stiffer aggregate type. Creep also decreases as the water-to-cement ratio is reduced. Creep also depends on the environment. It increases as the relative humidity decreases. Creep is also greater in thin members with large surface-area-to-volume ratios, such as slabs. However, the dependence of creep on both the relative humidity and the size and shape of the specimen decreases as the concrete strength increases. Near the surface of a member, creep takes place in a drying environment and is therefore greater than in regions remote from a drying surface. In addition to the relative humidity, creep is dependent on the ambient temperature. A rise in temperature increases the deformability of the cement paste and accelerates drying, and thus increases creep. The dependence of creep on temperature is more pronounced at elevated temperatures and is far less signiﬁcant for temperature variations between 0◦ C and 20◦ C. However, creep in concrete at a mean temperature of 40◦ C is perhaps 25 per cent higher than that at 20◦ C (Ref. 9). In addition to the environment and the characteristics of the concrete mix, creep depends on the loading history, in particular the magnitude and duration of the stress and the age of the concrete when the stress was ﬁrst applied. The age of the concrete, τ 0 , when the stress was ﬁrst applied has a marked inﬂuence on the ﬁnal magnitude of creep. Concrete loaded at an early age creeps more than concrete loaded at a later age. Concrete is therefore a time-hardening material, although even in very old concrete the tendency to creep never entirely disappears (Ref. 10). When the sustained concrete stress is less than about 0.5 fc , creep is approximately proportional to the stress and is known as linear creep. At higher stress levels creep increases at a faster rate and becomes non-linear with respect to stress. This nonlinear behaviour of creep at high stress levels is thought to be related to an increase in micro-cracking. Compressive stresses rarely exceed 0.5 fc in concrete structures at service loads, and creep may be taken as proportional to stress in most situations in the design for serviceability. In this book, the effects of non-linear creep at high stress levels are not examined.

Time-dependent deformation 7 1.2.2 Creep components To best understand the physical nature of creep and to describe its characteristics, creep strain is often subdivided into several components. In Fig. 1.2a, the creep strain produced by the compressive stress history of Fig. 1.2b is shown. Under sustained stress σo , creep increases at a decreasing rate. When the stress is removed at time τ1 , there is no sudden change in creep strain, but a gradual reduction occurs with time as shown. There is of course a sudden change in the total strain at τ1 due to the elimination of instantaneous strain. A portion of the creep strain is recoverable, while a usually larger portion is irrecoverable or permanent. The recoverable part of creep is often referred to as the delayed elastic strain, εcr.d (t). This delayed elasticity is thought to be caused by the elastic aggregate acting on the viscous cement paste after the applied stress is removed. If a concrete specimen is unloaded after a long period under load, the magnitude of the recoverable creep is in the order of 40–50 per cent of the elastic strain (between 10 and 20 per cent of the total creep strain). Although the delayed elastic strain is observed only as recovery when the load is removed, it is generally believed to be of the same magnitude under load and to develop rapidly in the period immediately after loading. Rüsch et al. (Ref. 8) suggest that the shape of the delayed elastic strain curve is independent of the age or dimensions of the specimen and is unaffected by the composition of the concrete. The majority of creep strain is irrecoverable and is often referred to as ﬂow, ε cr.f (t). The ﬂow component of creep is sometimes further subdivided into rapid initial ﬂow, εcr.ﬁ (t), that occurs in the ﬁrst 24 hours after loading, and the remaining ﬂow that develops gradually with time (Ref. 9). The rapid initial ﬂow is irrecoverable and highly dependent on the age at ﬁrst loading, that is, on the degree of hydration. The younger concrete is when ﬁrst loaded, the higher ε cr.ﬁ (t). The remaining ﬂow that occurs after the ﬁrst day under load is dependent on the relative humidity and, as discussed earlier, may be divided into a basic ﬂow component εcr.fb (t) and a drying ﬂow component εcr.fd (t). The drying ﬂow is the additional irrecoverable creep that occurs when the specimen is loaded in a drying environment. The basic ﬂow ε cr.fb (t) depends on the composition of the concrete mix (aggregate type, size and quantity, concrete strength, etc.) and the age of the concrete at the time of loading. The drying ﬂow εcr.fd (t) depends on the moisture content and gradient, and the size and shape of the specimen. In structural analysis, it is unusual to subdivide the ﬂow component of creep into all of these sub-components. However, consideration of the recoverable and irrecoverable Creep strain

Recoverable creep, −ecr.d (t1)

ecr(t) ecr.f

Irrecoverable creep, ecr.f (t1) +ecr.d (a)

t0

t1

Time

t0

t1

Time

Stress s0 (b)

Figure 1.2 Recoverable and irrecoverable creep components.

8 Time-dependent deformation components of creep (i.e. the delayed elastic and ﬂow components, respectively) is appropriate and necessary if concrete is subjected to a time-varying stress history. 1.2.3 Effects of ageing In the previous sections, we saw that all sub-components of creep are affected to some extent by the degree of hydration, i.e. the age of the concrete at the time of ﬁrst loading, τ . Fig. 1.3 shows the effect of age at ﬁrst loading on the creep–time curves of identical specimens ﬁrst loaded at ages τ 0 , τ 1 and τ 2 . Although not proven, it is usually assumed that the creep strain εcr (t, τ ) approaches ∗ (τ ). All else being equal: a limiting value as time approaches inﬁnity, i.e. εcr (∞, τ ) = εcr ∗ ∗ (τi ) > εcr (τj ) εcr

τi < τj

provided

(1.5)

This time-hardening or ageing of concrete complicates the prediction of creep strain under time-varying stress histories. 1.2.4 The creep coefﬁcient, ϕ(t,τ ), and the creep function, J(t, τ ) The capacity of concrete to creep is usually measured in terms of the creep coefﬁcient, ϕ(t,τ ). In a concrete specimen subjected to a constant sustained compressive stress, σc (τ ), ﬁrst applied at age τ , the creep coefﬁcient at time t is the ratio of the creep strain to the instantaneous strain and is given by: ϕ(t, τ ) =

εcr (t, τ ) εe (τ )

(1.6)

Therefore, the creep strain at time t caused by a constant sustained stress σc (τ ) ﬁrst applied at age τ is: εcr (t, τ ) = ϕ(t, τ ) εe (τ ) = ϕ(t, τ )

σc (τ ) Ec (τ )

(1.7)

Creep strain, ecr(t,t)

where Ec (τ ) is the elastic modulus at time τ . For concrete subjected to a constant sustained stress, knowledge of the creep coefﬁcient allows the rapid determination of the creep strain at any time.

e*cr (t0) e*cr (t1) * ecr (t2)

t0

t1

t2

Time

Figure 1.3 Effect of age at ﬁrst loading on creep strains.

Time-dependent deformation 9 Since both the creep and instantaneous strain components are proportional to stress for compressive stress levels less than about 0.5 fc , the creep coefﬁcient ϕ(t,τ ) is a pure time function and is independent of the applied stress. The creep coefﬁcient increases with time at an ever-decreasing rate. As time approaches inﬁnity, the creep coefﬁcient ∗ (τ )/ε (τ ) that usually falls within is assumed to approach a ﬁnal value ϕ ∗ (τ ) = εcr e the range 1.5–4.0. This ﬁnal creep coefﬁcient is a useful measure of the capacity of concrete to creep. Since creep strain depends on the age of the concrete at the time of ﬁrst loading, so too does the creep coefﬁcient. A family of creep coefﬁcient versus time curves may be drawn that are similar to the creep–time curves shown in Fig. 1.3. Another frequently used time function is known as speciﬁc creep, C(t,τ ), and is the proportionality factor relating stress to linear creep, i.e.: εcr (t, τ ) = C(t, τ ) σc (τ )

or C(t, τ ) =

εcr (t, τ ) σc (τ )

(1.8)

C(t, τ ) is the creep strain at time t produced by a sustained unit stress ﬁrst applied at age τ . The relationship between the creep coefﬁcient and speciﬁc creep can be obtained from Eqs 1.6 and 1.8: ϕ(t, τ ) = C(t, τ ) Ec (τ )

(1.9)

The sum of the instantaneous and creep strains at time t produced by a sustained unit stress applied at τ is deﬁned as the creep function, J(t, τ ), and is given by: J (t, τ ) =

1 1 + C(t, τ ) = [1 + ϕ(t, τ )] Ec (τ ) Ec (τ )

(1.10)

The stress-produced strains (i.e. the instantaneous plus creep strains) caused by a constant sustained stress σ c (τ ) ﬁrst applied at age τ (also called the stress-dependent strains) may therefore be determined from: εe (t) + εcr (t, τ ) = J(t, τ )σc (τ ) =

σc (τ ) σc (τ ) [1 + ϕ(t, τ )] = Ec (τ ) Ee (t, τ )

(1.11)

where Ee (t, τ ) is known as the effective modulus and is given by: Ee (t, τ ) =

Ec (τ ) [1 + ϕ(t, τ )]

(1.12)

The variation with time of the creep strain caused by a constant sustained stress σc (τ0 ) (≡σ c0 ) is shown in Fig. 1.4. In the remainder of this book, the creep coefﬁcient and the creep function are used to mathematically deﬁne and quantify creep. 1.2.5 The principle of superposition Because the load-dependent strains in concrete at service loads are proportional to stress, the principle of superposition is frequently used to estimate the deformation

10 Time-dependent deformation sc(t)

ecr(t, t0)

sc(t0)

j(t, t0) sc(t0)/Ec(t0) t0 Time (a) Constant stress history

t0 Time (b) Creep strain versus time

Figure 1.4 Creep strain produced by a constant sustained stress.

caused by a time-varying stress history. The principle of superposition was ﬁrst applied to concrete by McHenry (Ref. 11) who stated that the strain produced by a stress increment applied at any time τ i is not affected by any stress applied either earlier or later. This principle is illustrated in Fig. 1.5. For increasing stress histories, such as that shown in Fig. 1.5c, the principle of superposition agrees well with experimental observations. The creep curve produced by the increasing stress history is assumed to be equal to the sum of the creep curves produced by each stress increment acting independently. However, for decreasing stress histories, the principle of superposition overestimates creep recovery, as shown in Fig. 1.5d. This can easily be seen when one divides creep into delayed elastic and ﬂow components. The principle of superposition incorrectly assumes that at any time t τ1 , the delayed elastic strain that develops between τ0 and τ1 , εcr.d (τ1 , τ0 ), is equal to the Curve (a)

ecr (t)

sc

j(t,t0) sc (t0 )/Ec(t0)

sc(t0)

(a)

t0

Time

t0

Time

ecr (t)

sc

Curve (b)

sc(t1) = sc(t0)

sc(t1)

j(t,t1) sc(t1)/Ec(t1)

(b)

t1

t1

Time

Time

ecr (t) sc 2sc(t0 )

Curve (c) = Curve (a) + Curve (b)

sc(t0 )

(c)

t0

t1

t0

Time

t1

Time

ecr (t)

Actual

sc sc(t0 )

(d)

Curve (d) = Curve (a) − Curve (b) t0

t1

Time

t0

t1

Time

Figure 1.5 The principle of superposition of creep strains.

Time-dependent deformation 11 creep strain at time t produced by σc (τ1 ) = σc (τ0 ) applied at τ1 (i.e. εcr (t, τ1 )). In fact, εcr.d (τ1 , τ0 ) is signiﬁcantly less than εcr (t, τ1 ). Nevertheless, for most practical purposes, the principle of superposition provides a good approximation of the time-dependent strains in concrete caused by a time-varying stress history. To illustrate the principle of superposition, consider the stress history shown in Fig. 1.6a consisting of two stress increments σ c (τ 0 ) and σ c (τ 1 ) applied at times τ 0 and τ 1 , respectively. In this case, two creep coefﬁcients ϕ(t, τ 0 ) and ϕ (t, τ 1 ) are required to determine the creep strain at any time t > τ 1 . Graphs of the two creep coefﬁcients versus time curves are shown in Fig. 1.6b and the corresponding creep function versus time curves are given in Fig. 1.6c. According to the principle of superposition, the total stress-dependent strain in concrete at time t (elastic plus creep strains) can be written as: εe (t) + εcr (t) = =

σc (τ0 ) σc (τ1 ) [1 + ϕ(t, τ0 )] + [1 + ϕ(t, τ1 )] Ec (τ0 ) Ec (τ1 ) 1 σc (τi ) i=0

Ec (τi )

[1 + ϕ(t, τi )]

(1.13)

where the argument τ has been eliminated from the elastic strain εe (t) and creep strain εcr (t) as the stress history varies with time. This notation is more appropriate for realistic time-varying stress histories and will be used throughout the remainder of the book. Eq. 1.13 can also be written in terms of creep functions as: εe (t) + εcr (t) = J(t, τ0 )σc (τ0 ) + J(t, τ1 )σc (τ1 ) =

1

J(t, τi )σc (τi )

(1.14)

i=0

The variations with time of the elastic and creep deformations are plotted in Fig. 1.7. A useful graphic interpretation of the elastic and creep deformations is shown in Fig. 1.8, where Figs 1.6a and 1.6c have been combined. The stress increments of Fig. 1.6a are plotted on the horizontal axis of Fig. 1.8b and Fig. 1.6c has been reproduced for ease of reference in Fig. 1.8a. At any time t > τ1 the area under the sc(t) sc(t1)

Dsc(t1)

sc(t0)

Dsc(t0) t1 t0 Time (a) Stress history consisting of two stress increments j(t,t)

J(t,t) j (t,t0)

J(t,t0) J(t,t1)

j(t,t1) t0

t1

(b) Creep coefficient

Time

t0

t1

Time

(c) Creep function

Figure 1.6 Creep coefﬁcients and creep functions associated with two stress increments.

12 Time-dependent deformation

ee(t)+ecr(t)

J(t,t0) Δsc(t0) + J(t,t1) Δsc(t1)

ecr(t)

j(t,t0) Δsc(t0)/Ec(t0)

J(t,t0) Δsc(t0)

t0

j(t,t0) Δsc(t0) /Ec(t0) + j(t,t1) Δsc(t1) /Ec(t1)

t1

t0

Time

(a) Elastic and creep deformations

t1

Time

(b) Creep deformation

Figure 1.7 Creep and elastic deformations due to two stress increments (Fig. 1.6a).

curve of Fig. 1.8b represents the actual stress-dependent deformation (sum of elastic and creep strains) at time t as deﬁned in Eq. 1.14. Consider the stress history shown in Fig. 1.9a. By dividing the time under load into n time steps, the continuously varying stress may be approximated by a series of small stress increments applied at the end of each time step. The stress-produced strains at time t are given by: εe (t) + εcr (t) =

n σc (τi ) i=0

Ec (τi )

[1 + ϕ(t, τi )] =

n

J(t, τi )σc (τi )

(1.15)

i=0

and a different creep coefﬁcient is required for each small stress increment, σ (τ i ). According to the principle of superposition, the total strain in concrete at time t subjected to the stress history shown in Fig. 1.9 is obtained by summing the stress-produced strains and the shrinkage strain: ε(t) = εe (t) + εcr (t) + εsh (t) ε(t) =

n

J(t, τi )σc (τi ) + εsh (t) =

i=0

n σc (τi ) i=0

Ec (τi )

+

n σc (τi )ϕ(t, τi ) i=0

J(t2,t)

J(t,t)

J(t2,t0)

J(t2,t1)

J(t2,t1)

J(t2,t0)

t0

t1 (a) Creep function

t2

Time

Ec (τi )

+ εsh (t) (1.16)

J(t2,t0) Ds(t0)

J(t2,t1) Ds (t1)

Ds(t0) Ds(t1) (b) Elastic plus creep deformations

Figure 1.8 Graphical representation of elastic plus creep deformation at time τ2 caused by two previous stress increments.

Time-dependent deformation 13 Creep function J(t,t0)

Stress

Hatched area = stress-produced strain (when stress increments are infinitesimally small)

Dsc(ti) sc(t)

i-th time interval Dti

Dsc(t0) t0 t1 t2

ti−1 ti Time

J(t,tn) sc(t0) Stress

t=tn

(a) Time-varying stress history

sc(tn)

(b) Stress-produced strains

Figure 1.9 Time-varying stress history and stress-produced strains.

In the limit, considering inﬁnitesimal stress increments dσ c (τ ), the summation included in Eq. 1.16 can be replaced by an integral: t

t J(t, τ )dσc (τ ) + εsh (t) =

ε(t) = τ0

τ0

1 + ϕ(t, τ ) dσc (τ ) + εsh (t) Ec (τ )

(1.17)

Equation 1.17 is referred to as the integral-type creep law (Ref. 12). The integral in Eq. 1.17 for the stress-produced strains is the area under the graph of creep function versus concrete stress in Fig. 1.9b. The stress at a point in a concrete structure under constant load often decreases with time as a result of creep. Consider the time-varying stress history shown in Fig. 1.10a where the initial stress σ c (τ 0 ) is compressive and decreases with time (i.e. all subsequent stress increments σ c (τ i ) are tensile). Notwithstanding the inaccuracies when the principle of superposition is applied to a decreasing stress history (mentioned previously), the stress produced strain may still be obtained using Eqs 1.16 or 1.17, with the integral in Eq. 1.17 represented by the hatched area under the curve in Fig. 1.10b. Creep function

Stress J(t,t0)

sc(t0) sc(t) Dsc(ti)

J(t,tn) i-th time interval t0 t1 t2

ti−1 ti Time

t = tn

(a) Gradually decreasing stress history

Hatched area = stress-produced strain (when stress increments are infinitesimally small) sc(tn) Stress

sc(t0)

(b) Stress-produced strain

Figure 1.10 Gradually decreasing stress history and stress-produced strain.

14 Time-dependent deformation The main disadvantage of the method of superposition, apart from its reduced accuracy when applied to a decreasing stress history, is the large amount of creep data required. Nevertheless, in a more general sense, the principle of superposition is relied upon in many ﬁelds of structural engineering and the analysis for time effects in concrete structures is no exception. 1.2.6 Tensile creep The previous discussions have been concerned with the creep of concrete in compression. However, the creep of concrete in tension is also of interest in a number of practical situations; for example, when studying the effects of restrained or differential shrinkage. Tensile creep also plays a signiﬁcant role in the analysis of suspended reinforced concrete slabs at service loads where stress levels are generally low and typically much of the slab is initially uncracked. Comparatively little attention has been devoted to the study of tensile creep (Ref. 1) and only limited experimental results are available in the literature, e.g. Ref. 13. Some researchers have multiplied the creep coefﬁcients measured for compressive stresses by factors in the range of 1 to 3 to produce equivalent coefﬁcient describing tensile creep (e.g. Refs 14 and 15). It appears that the mechanisms of creep in tension are different to those in compression. The magnitudes of both tensile and compressive creep increase when loaded at earlier ages. However, the rate of change of tensile creep with time does not decrease in the same manner as for compressive creep, with the development of tensile creep being more linear (Ref. 13). Drying tends to increase tensile creep in a similar manner to compressive creep and tensile creep is in part recoverable upon removal of the load. Further research is needed to provide clear design guidance. In this book, it is assumed that the magnitude and rate of development of tensile creep are similar to that of compressive creep at the same low stress levels. 1.2.7 The effects of creep on structural behaviour Creep is the time-dependent strain that develops in concrete due to sustained stress. When a loaded concrete member is unrestrained by steel reinforcement or by the external support conditions (such as a statically determinate plain concrete member), creep causes little more than an increase in deformations. The internal actions caused by imposed deformations in an indeterminate structure are proportional to stiffness. Due to creep, the internal actions caused by imposed deformations decrease with time in all concrete structures whether they are plain or reinforced. On the other hand, creep will not cause redistribution of loadinduced internal actions provided the creep characteristics are uniform throughout the structure. The effect of creep in this case is similar to a gradual and uniform change in the elastic modulus. Such a situation exists in an uncracked plain concrete member, if it is assumed that the creep characteristics of concrete in tension are the same as those in compression (which is a usual although not strictly correct assumption). The same is true in an uncracked reinforced concrete structure provided the reinforcement is symmetrical on each cross-section and uniform throughout the structure.

Time-dependent deformation 15 When portions of a statically indeterminate structure are made of different materials or of concrete with a different composition or age, and hence different creep characteristics, creep causes a redistribution of the load-induced internal actions. The internal actions are redistributed from the regions with the higher creep rate to the regions with the lower creep rate. In practical reinforced concrete ﬂexural members, the creep characteristics are rarely uniform throughout. Some regions are usually cracked and some are not. Reinforcement quantities usually vary along the length of the member and sections are seldom symmetrically reinforced. Nevertheless, the redistribution caused by creep of the load-induced bending moments and shear forces in statically indeterminate members is generally small and is quite often neglected in design. Creep can dramatically change the stress distribution on a reinforced concrete section. For example, stresses caused by shrinkage or temperature changes are relieved by creep. Creep also causes a redistribution of stresses between concrete and the bonded reinforcement on a cross-section. For example, consider a reinforced concrete column section subjected to a constant sustained axial compressive load. The concrete and steel are bonded together so that at any time compatibility requires that the concrete and steel strains are identical. As the compressive concrete creeps (contracts), the steel is compressed and the compressive stress in the steel gradually increases. Shrinkage causes a similar effect. Equilibrium requires that the increase in the compressive force in the steel is balanced by an equal and opposite tensile force on the concrete. Therefore, the compressive stress in the concrete reduces with time, while the steel stress increases rapidly. Load is thus transferred from the concrete to the steel, with the proportion of the external load carried by the reinforcement increasing with time. Fig. 1.11 shows the typical variation in compressive stresses in the concrete and steel caused by creep on the cross-section of an axially loaded reinforced concrete column subjected to a constant sustained compressive force, P. It is quite common, in fact, for the stress in the longitudinal reinforcement in typically proportioned reinforced concrete columns to be close to the yield stress at service loads, 300

sc = 10.0 MPa

10

ss = 242 MPa 250

Steel stress

Concrete stress 200 sc = 72.2 MPa

8 6

150

300 mm P = 1000 kN Ec = 25 GPa Es = 200 GPa j*(t) = 3.0

4

300 mm ss = 80.0 MPa

+

2

100

50

Steel compressive stress (MPa)

Concrete compressive stress (MPa)

12

As = 1500 mm2 0 0

t

Time (days)

0 10,000

Figure 1.11 Variation of stresses with time due to creep on a symmetrically reinforced axially loaded column section.

16 Time-dependent deformation due to the effects of creep and shrinkage (particularly for low-strength steel grades). The use of closely spaced lateral reinforcement in the form of closed ties or helices to prevent these highly stressed bars from buckling is therefore essential at the service load condition and not just at the ultimate load condition. The gradual development of creep strain on a reinforced concrete beam section causes an increase of curvature, as shown in Fig. 1.12, and a consequent increase in the beam deﬂection. For a plain concrete member, the increase in curvature is proportional to the creep coefﬁcient (i.e. the increase in curvature is proportional to the uniform increase in strain at every point on the section). For an uncracked, singly reinforced section (Fig. 1.12a), creep is restrained in the tensile zone by the reinforcement. Depending on the quantity of steel, the increase in curvature due to creep is proportional to a large fraction of the creep coefﬁcient (usually between 0.6ϕ(t) and 0.9ϕ(t)). On a cracked, singly reinforced beam section (Fig. 1.12b), the initial curvature is comparatively large and the cracked tensile concrete below the neutral axis can be assumed to carry no stress and therefore does not creep. Creep in the compression zone causes a lowering of the neutral axis and a consequent reduction in the compressive stress level. Creep is slowed down as the compressive stress reduces, and the increase in curvature is proportional to a small fraction of the creep coefﬁcient (usually less than one quarter). The relative increase in deﬂection caused by creep is therefore greater in an uncracked beam than in a cracked beam, although the total deﬂection in the cracked beam is signiﬁcantly greater. In prestressed concrete construction, in addition to causing increases in deﬂection (and camber), both creep and shrinkage cause shortening of the concrete member that in turn causes shortening of the prestressing tendons and a consequent reduction in the prestressing force. This loss of prestress may adversely affect the performance of the member at service loads and should be accounted for in its design. etop ≈etop(1+j) k0 k (t)

Ms

Time t Instantaneous

Section

Elevation

Strain

(a) Uncracked cross-section etop 0.7: Wire or strand: k5 = 5γ – 2.5 Alloy steel bars: k5 = (50γ – 29)/6

0 0.4 0.5 0.6 0.7 0.8 Stress in tendon as a proportion of fp, that is, g = sp,init /fp

Figure 2.4 Coefﬁcient, k5 (Ref. 2).

Creep in the prestressing steel may also be deﬁned in terms of a creep coefﬁcient ϕp (t, σp,init ) rather than as a relaxation loss. If the creep coefﬁcient for the prestressing steel ϕp (t, σp,init ) is the ratio of creep strain in the steel to the initial elastic strain, then the ﬁnal creep coefﬁcients for low relaxation wire, strand and bar are also given in Table 2.7 and may be approximated using Eq. 2.12. ϕp (t, σp,init ) =

R 1−R

(2.12)

Note that the creep of high-strength steels is non-linear with respect to stress. As has already been emphasised, creep (relaxation) of the prestressing steel depends on the stress level. In a prestressed concrete member, the stress in a tendon is gradually reduced with time as a result of creep and shrinkage in the concrete. This gradual reduction of stress results in a reduction of creep in the steel and hence smaller relaxation losses. To determine relaxation losses in a concrete structure therefore, the ﬁnal relaxation loss obtained from Eq. 2.11 (or Table 2.7) should be multiplied by a reduction factor, λr , that accounts for the time-dependent shortening of the concrete due to creep and shrinkage. The factor λr depends on the creep and shrinkage characteristics of the concrete, the initial prestressing force, and the stress in the concrete at the level of the steel, and can be determined by iteration (Ref. 17). However, because relaxation losses in modern prestressed concrete Table 2.7 Long-term relaxation losses and corresponding ﬁnal creep coefﬁcients for low relaxation wire, strand and bar (T = 20◦ C) Type of tendon

Wire Strand Bar

Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init ) Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init ) Relaxation loss, R(%) Creep coefﬁcient, ϕp (t, σp,init )

Tendon stress as a proportion of fp 0.6

0.7

1.9 0.019 2.4 0.025 3.7 0.039

2.8 0.029 3.5 0.036 5.6 0.059

0.8 4.2 0.044 5.3 0.056 10.3 0.115

36 Material properties structures (employing low-relaxation steels) are relatively small, it is usually sufﬁcient to take λr ≈ 0.8. When elevated temperatures exist during curing (i.e. steam curing), relaxation is increased and occurs rapidly during the curing cycle. For low relaxation steel in a concrete member subjected to an initial period of steam curing, it is recommended that the design relaxation be taken signiﬁcantly greater than the value given by Eq. 2.11 (calculated with T = 20◦ C).

2.3 References 1. Gilbert, R.I. (2002). Creep and shrinkage models for high strength concrete – proposals for inclusion in AS3600. Australian Journal of Structural Engineering, IEAust, 4(2), 95–106. 2. Standards Australia (2009). Australian Standard for Concrete Structures, AS3600–2009. Sydney. 3. ACI Committee 209 (2008). Guide for modeling and calculating shrinkage and creep in hardened concrete (ACI 209.2R-8). American Concrete Institute, Farmington Hills, Michigan. 4. ACI Committee 209 (1992). Prediction of creep, shrinkage, and temperature effects in concrete structures (ACI 209R-92). American Concrete Institute, Farmington Hills, Michigan. 5. Bazant, Z.P. and Baweja, S. (2000). Creep and shrinkage prediction model for analysis and design of concrete structures: model B3. The Adam Neville Symposium: Creep and Shrinkage – Structural Design Effects, ACI SP-194. American Concrete Institute, Farmington Hills, Michigan, 236–260. 6. Bazant, Z.P. and Baweja, S. (1995). Creep and shrinkage prediction model for analysis and design of concrete structures – model B3. Materials and Structures, 28, 357–365. 7. Comité Euro-International du Béton (1993). CEB-FIB Model Code 1990: Design Code. Thomas Telford, London. 8. Comité Euro-International du Béton (1999). Structural concrete – Textbook on behaviour, design and performance – Volume 2: Basis of design. Fib Bulletin No. 2, Federation Internationale du Béton, Lausanne, Switzerland, 37–52. 9. British Standard (2004). BS EN 1992, Eurocode 2: Design of concrete structures - Part 1-1: general rules and rules for buildings. British Standards Institute, Milton Keynes. 10. Gardner, J. and Lockman, M.J. (2001). Design provisions for drying shrinkage and creep of normal-strength concrete. ACI Materials Journal, 98(2), 159–167. 11. Comité Euro-International du Béton (1984). CEB Design manual on structural effects of time-dependent behaviour of concrete. M.A. Chiorino (ed.), Georgi Publishing, SaintSaphorin, Switzerland. 12. Pauw, A. (1960). Static Modulus of Elasticity of Concrete as Affected by Density. ACI Journal, 57(6), 679–687. 13. Gilbert, R.I. (1988). Time Effects in Concrete Structures. Elsevier Science Publishers, Amsterdam. 14. Bazant, Z.P. and Li, G.-H. (2008). Unbiased statistical comparison of creep and shrinkage prediction models. ACI Materials Journal, 105(6), 610–619. 15. Chiorino, M.A. (2005). A rational approach to the analysis of creep structural effects. Shrinkage and Creep of Concrete, SP-227, American Concrete Institute, Farmington Hills, Michigan, 107–141. 16. Brooks, J.J. (2005). 30-year creep and shrinkage of concrete. Magazine of Concrete Research, 57(9), 545–556. 17. Ghali, A., Favre, R., and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London.

3

Design for serviceability Deﬂection and crack control

3.1 Introduction The tensile capacity of concrete is usually neglected when calculating the strength of a reinforced concrete member, even though the concrete continues to carry tensile stress between the cracks due to the transfer of forces from the tensile reinforcement to the concrete through bond. This contribution of the tensile concrete is known as tension stiffening and it affects the stiffness of the member after cracking and hence its deﬂection and the width of the cracks. Reinforced concrete members often contain relatively small quantities of tensile reinforcement, in some situations close to the minimum amount permitted by the relevant building code. This is particularly so in the case of ﬂoor slabs. For such members, the ﬂexural rigidity of a fully cracked cross-section (Ec Icr ) is many times smaller than that of an uncracked cross-section (Ec Iuncr ) and tension stiffening contributes greatly to the member’s stiffness after cracking. In structural design, deﬂection and crack control at service load levels are usually the governing considerations and accurate modelling of the stiffness after cracking is required. In-service deﬂections depend primarily on the properties of the concrete and these are often not known reliably at the design stage. The non-linear behaviour that complicates serviceability calculations is due to cracking, tension stiffening, creep and shrinkage of the concrete. Of these, shrinkage is perhaps the most problematic. Shrinkage may cause time-dependent cracking that reduces member stiffness and gradually reduces the beneﬁcial effects of tension stiffening. It results in a gradual widening of existing cracks and, in ﬂexural members, a signiﬁcant increase in deﬂections with time. The problem is particularly difﬁcult in the case of slabs that are typically shallow, with relatively large span to depth ratios, and are therefore deﬂection sensitive. The ﬁnal deﬂection of a slab depends very much on the extent of initial cracking which, in turn, depends on the construction procedure (shoring and re-shoring), the amount of early shrinkage, the temperature gradients in the ﬁrst few weeks after casting, the degree of curing and so on. Many of these parameters are, to a large extent, outside of the control of the designer. In ﬁeld measurements of the deﬂection of many identical slab panels (Refs 1 and 2), large variability was reported. Deﬂections of identical panels after one year differed by over 100 per cent in some cases. These differences can be attributed to the different conditions (both in terms of load and environment) that existed in the ﬁrst few weeks after the casting of each slab.

38 Design for serviceability Serviceability failures of concrete structures involving excessive cracking and/or excessive deﬂection are relatively common. Numerous cases have been reported of structures that complied with the local code requirements but still deﬂected or cracked excessively (Refs 1–3). In many of these cases, shrinkage of the concrete was primarily responsible or, probably more precisely, failure to adequately account for shrinkage (and creep) in the design was primarily responsible. The need for a more reliable deﬂection calculation procedure has been exacerbated by the introduction, in recent years, of higher strength reinforcing steels. The use of higher strength steel usually means that less steel is required for strength and, consequently, less stiffness is available after cracking, leading to greater deﬂection and wider cracks under service loads. Design for serviceability has increasingly assumed a more prominent role in the design of both beams and slabs. This chapter describes the behaviour of reinforced concrete elements under service loads and outlines the simpliﬁed approaches for deﬂection and crack control that are speciﬁed in modern design codes, including ACI 318-08 (Ref. 4), Eurocode 2 (Refs 5 and 6) and AS 3600-2009 (Ref. 7). The limitations of these simpliﬁed approaches are discussed and the need for the more reﬁned methods of analysis at the serviceability limit states that are described in subsequent chapters is demonstrated.

3.2 Design objectives and criteria The broad design objective for a concrete structure is that it should satisfy the needs for which it was contrived. In doing so, the structural designer must ensure that it is safe and serviceable, so that the chance of it failing during its design lifetime is sufﬁciently small. Structural failure can take a variety of forms. The structure must be strong enough and sufﬁciently ductile to resist, without collapse, the overloads and environmental extremes that may be imposed upon it. It must also perform satisfactorily under day-to-day service loads without deforming, cracking or vibrating excessively. The two primary structural design objectives are therefore strength and serviceability. Other structural design objectives are stability and durability – a structure must be stable and resist overturning or sliding; reinforcement must not corrode; concrete must resist abrasion and spalling, and the structure must not suffer a signiﬁcant reduction of strength or serviceability with time. Another non-structural, but important, objective is aesthetics and, of course, an overarching design objective is economy. Ideally, the structure should be in harmony with, and enhance, the environment and this often requires collaboration between the structural engineer, environmental engineer and architect. The aim is to achieve, at minimum cost, an aesthetically pleasing and functional structure that satisﬁes the required structural objectives. In order for design calculations to proceed for a particular structure, the design objectives must be translated into quantitative terms called design criteria. For example, the designer needs to determine the maximum acceptable deﬂection for a particular beam or slab, or the maximum crack width that can be tolerated in a concrete ﬂoor or wall. Also required are minimum numerical values for the strength of individual elements or connections. It is also necessary to identify and quantify all of the loads or actions that will be applied to the structure and the probability of their occurrence. The design criteria are speciﬁed in codes of practice and provide a suitable margin of safety (called the safety index) against a structure becoming unﬁt for service in any way.

Design for serviceability

39

The speciﬁc form of the design criteria depends on the philosophy and method of design adopted by the relevant code and the manner in which the inherent variability in both the load and the structural performance is considered. Modern design codes for structures have generally adopted the limit states method of design, whereby a structure must be designed to simultaneously satisfy a number of different limit states or design requirements, including adequate strength and serviceability. Minimum performance criteria are speciﬁed for each of these limit states and any one may become critical and govern the design of a particular member. If a structure ceases to fulﬁl its intended function in any way, it is said to enter a limit state. Each possible mode of failure is a limit state. For each limit state, codes of practice specify both load combinations and methods of predicting the actual structural performance that together ensure an acceptably low probability of failure, depending on the consequences and cost of the failure. For the strength limit states, the consequences of failure are high and so the probability of failure must be very low. For the serviceability limit states, such as excessive deﬂection or excessive cracking, the consequences of failure are not as great and a higher probability of failure is justiﬁable. Design for the serviceability limit states involves making reliable predictions of the time-dependent deformation of the concrete structure. This is complicated by the nonlinear material behaviour of concrete, caused mainly by cracking, tension stiffening, creep and shrinkage. This book deals primarily with the inclusion of these material non-linearities in the analysis of concrete structures, and so it is primarily concerned with designing for serviceability. In order to satisfy the serviceability limit states, a concrete structure must be serviceable and perform its intended function throughout its working life. Excessive deﬂection should not impair the function of the structure or be aesthetically unacceptable. Excessive deﬂection should also not cause unintended load paths, such as occurs when a deﬂecting slab begins to bear on a non-load-bearing partition. Cracks should not be unsightly or wide enough to lead to durability problems and vibration should not cause distress to the structure or discomfort to its occupants.

3.3 Design actions In the design of concrete structures for the serviceability limit states, the internal actions and deformations that arise from appropriate combinations of the day-to-day service loads should be considered, including, where applicable: dead load (G); live load (Q); wind load (W); prestress (P); earthquake load (Feq ); earth pressure (Fep ); liquid pressure (Flp ); and snow load (Fs ). In addition, any accidental loading and loads arising during construction should be considered where they may adversely affect the various limit states’ requirements. Other actions that may affect the serviceability of the structure include, creep of concrete, shrinkage of concrete and other imposed deformations, such as may result from temperature changes and gradients, support settlements and foundation movements. Dead loads are generally deﬁned as those loads imposed by both the structural and non-structural components of a structure. Dead loads include the self-weight of the structure and the forces imposed by all walls, ﬂoors, roofs, ceilings, permanent partitions, service machinery and other permanent construction. Dead loads are usually permanent, ﬁxed in position and can be estimated reasonably accurately from the mass of the relevant material or type of construction. For example, normal weight

40 Design for serviceability concrete weighs about 24 kN/m3 . Lightweight reinforced concrete weighs between 15 and 20 kN/m3 . Live loads are the loads that are attributed to the intended use or purpose of the structure and are generally speciﬁed by regional or national codes and speciﬁcations, such as Refs 8–13. The speciﬁed live load depends on the expected use or occupancy of the structure and usually includes allowances for impact and inertia loads (where applicable) and for possible overload. Both uniformly distributed and concentrated live loads are normally speciﬁed. The magnitude and distribution of the actual live load is never known accurately at the design stage, and it is by no means certain that the speciﬁed live load will not be exceeded at some stage during the life of the structure. Live loads may or may not be present at any particular time; they are not constant and their position can vary. Although part of the live load is transient, some portion may be permanently applied to the structure and have effects similar to dead loads. Live loads also arise during construction due to the stacking of building materials, the use of particular equipment or the construction procedure (such as the loads induced by ﬂoor-to-ﬂoor propping in multi-storey construction). The speciﬁed wind, earthquake, snow and temperature loads depend on the geographical location and relative importance of the structure (the mean return period). Wind loads also depend on the surrounding terrain and the height of the structure above the ground. These environmental loads are also usually speciﬁed by regional or national codes and speciﬁcations, such as Refs 13–16. The design loads to be used in serviceability calculations are the day-to-day service loads and these may be considerably less than the speciﬁed loads. For example, the speciﬁed live load, Q, has a built-in allowance for overload and impact. There is a low probability that it will be exceeded. It is usually not necessary, therefore, to ensure acceptable deﬂections and crack widths under the full speciﬁed loads. Use of the actual load combinations under normal conditions of service – the expected loads – is more appropriate. Often, codes of practice differentiate between the speciﬁed (or characteristic) loads and the expected loads. Depending on the type of structure, the expected loads may be signiﬁcantly less than the speciﬁed loads. If the aim of the serviceability calculation is to produce a best estimate of the likely behaviour, then expected loads should be considered. Often the magnitudes of the expected loads are not deﬁned and are deemed to be a matter of engineering judgment. In some codes, serviceability load factors (ψ ≤ 1.0) are nominated to determine the expected load from the speciﬁed load for both short-term (ψ1 Q) and long-term loading (ψ2 Q). If the aim is to satisfy a particular serviceability limit state and the consequences of failure to do so are high, then the speciﬁed loads may be more appropriate. Once again, the decision should be based on engineering judgment and experience. With regard to dead loads, the expected and speciﬁed values are the same and therefore the speciﬁed dead load should be used in all serviceability calculations. For live loads, the expected values should be used when a best estimate is required. For building structures, the expected live load for short-term serviceability load combinations is usually about 70 per cent of the speciﬁed live load for dwellings (i.e. ψ1 = 0.7), 60 per cent for retail areas, 50 per cent for ofﬁces and parking areas and 100 per cent for storage areas. For bridges, the live load for short-term serviceability load combinations is usually taken to be about 70 per cent of the speciﬁed live load for spans of less than about 10 m, reducing to 50 per cent for spans greater than 100 m.

Design for serviceability

41

For long-term serviceability calculations, the following percentages of the speciﬁed live load are usually considered as permanent or sustained (with the remainder being transitory in nature): 30 per cent for dwellings and retail stores (i.e. ψ2 = 0.3), 25 per cent for parking areas, 20 per cent for ofﬁces, and 50–80 per cent for storage areas. With the appropriate design actions for serviceability determined, the response of the structure must satisfy the relevant design criteria for deﬂection and crack control. These are usually also embodied in the codes of practice and are discussed in the following sections.

3.4 Design criteria for serviceability 3.4.1 Deﬂection limits The design for serviceability, particularly the control of deﬂections, is frequently the primary consideration when determining the cross-sectional dimensions of beams and ﬂoor slabs in concrete buildings. This is particularly so in the case of slabs, as they are typically thin in relation to their spans and are therefore deﬂection sensitive. It is stiffness rather than strength that usually controls the design of slabs, particularly in the cases of ﬂat slabs and ﬂat plates. Most concrete design codes, including ACI 318-08 (Ref. 4), Eurocode 2 (Ref. 6) and the Australian Standard AS 3600-2009 (Ref. 7), specify two basic approaches for deﬂection control. The ﬁrst and simplest approach is deﬂection control by the satisfaction of a minimum depth requirement or a maximum span-to-depth ratio (see Section 3.5). The second approach is deﬂection control by the calculation of deﬂection, where the deﬂection (or camber) is calculated using realistic models of material and structural behaviour. This calculated deﬂection should not exceed the deﬂection limits that are appropriate to the structure and its intended use. The deﬂection limits should be selected by the designer and are often a matter of engineering judgment. Codes of practice give general guidance for both the selection of the maximum deﬂection limits and the calculation of deﬂection. However, the simpliﬁed procedures for calculating the deﬂections of beams and slabs in most codes are necessarily design-oriented and simple to use, involving crude approximations of the complex effects of cracking, tension stiffening, concrete creep, concrete shrinkage and the load history (see Section 3.6). Generally, they have been developed and calibrated for simply-supported reinforced concrete beams (Ref. 17) and often produce inaccurate and non-conservative predictions when applied to lightly reinforced concrete slabs (Ref. 18). In addition, most existing code procedures do not provide real guidance on how to adequately model the time-dependent effects of creep and shrinkage in deﬂection calculations. There are three main types of deﬂection problem that may affect the serviceability of a concrete structure: 1 2 3

where excessive deﬂection causes either aesthetic or functional problems; where excessive deﬂection results in unintended load paths or damage to either structural or non-structural elements attached to the member; where dynamic effects due to insufﬁcient stiffness cause discomfort to occupants.

42 Design for serviceability Examples of deﬂection problems of type 1 include visually unacceptable sagging (or hogging) of slabs and beams and ponding of water on roofs. Type 1 problems are generally overcome by limiting the magnitude of the ﬁnal long-term deﬂection (here called total deﬂection) to some appropriately low value. The total deﬂection of a beam or slab in a building is usually the sum of the short-term and time-dependent deﬂections caused by the dead load (including self-weight), the prestress (if any), the expected in-service live load and the load-independent effects of shrinkage and temperature change. When the total deﬂection exceeds about span/200 below the horizontal, it may become visually unacceptable. Total deﬂection limits that are appropriate for the particular member and its intended function must be selected by the designer. For example, a total deﬂection limit of span/200 may be appropriate for the ﬂoor of a car park, but would be totally inadequate for a gymnasium ﬂoor that is required to remain essentially plane under service conditions and where functional problems arise at very small total deﬂections. AS 3600-2009 (Ref. 7) requires that a limit on the total deﬂection be selected that is appropriate to the structure and its intended use, but that limit should not be greater than span/250 for a span supported at both ends and span/125 for a cantilever (see Table 3.1). Examples of type 2 problems include deﬂection-induced damage to ceiling or ﬂoor ﬁnishes, cracking of masonry walls and other brittle partitions, improper functioning of sliding windows and doors, tilting of storage racking and so on. To avoid these problems, a limit must be placed on that part of the total deﬂection that occurs after the attachment of the non-structural elements in question, that is, the incremental deﬂection. This incremental deﬂection is the sum of the long-term deﬂection due to all of the sustained loads and shrinkage, the short-term deﬂection due to the transitory live load and the short-term deﬂection due to any dead load applied to the structure after the attachment of the non-structural elements under consideration, together with any temperature-induced deﬂection. For roof or ﬂoor construction supporting or attached to non-structural elements that are likely to be damaged by large deﬂection, ACI 318-08 (Ref. 4) limits the incremental deﬂection to span/480 (and span/240 when the non-structural elements are unlikely to be damaged by deﬂection). Incremental deﬂections of span/480 can, in fact, cause cracking in supported masonry walls, particularly when doorways or corners prevent arching and when no provisions are made to minimise the effect of movement. AS 3600-2009 limits the incremental deﬂection for members supporting masonry partitions or other brittle ﬁnishes to between span/500 and span/1000 depending on the provisions made to minimise the effect of movement (see Table 3.1). Eurocode 2 (Ref. 6) recommends limits on total (incremental) deﬂection of span/250 (span/500). Type 3 deﬂection problems include the perceptible springy vertical motion of ﬂoor systems and other vibration-related problems. Very little quantitative information for controlling this type of deﬂection problem is available in codes of practice. For a ﬂoor that is not supporting or attached to non-structural elements likely to be damaged by large deﬂection, ACI 318-08 (Ref. 4) places a limit of span/360 on the short-term deﬂection due to live load (and span/180 for a ﬂat roof). This limit provides a minimum requirement on the stiffness of members that may, in some cases, be sufﬁcient to avoid type 3 problems. Such problems are potentially the most common for prestressed concrete ﬂoors, where load balancing is often employed to produce a nearly horizontal ﬂoor under the sustained load and the bulk of the ﬁnal deﬂection is due to the transient

Design for serviceability

43

Table 3.1 Limits for calculated deﬂections of beams and slabs with effective span ef Type of member

Deﬂection to be considered

Deﬂection limitation for spans (Notes 2 and 3)

Deﬂection limitation for cantilevers (Note 5)

All members Members supporting masonry partitions

The total deﬂection The deﬂection that occurs after the addition or attachment of the partitions

ef /250 ef /500 where provision is made to minimise the effect of movement, otherwise ef /1000

Members supporting other brittle ﬁnishes

The deﬂection that occurs after the addition or attachment of the ﬁnish The imposed action (live load and dynamic impact) deﬂection Total deﬂection

Manufacturer’s speciﬁcation but not more than ef /500

ef /125 ef /250 where provision is made to minimise the effect of movement, otherwise ef /500 Manufacturer’s speciﬁcation but not more than ef /250

ef /800

ef /400

ef /500 where provision is made to minimize the effect of deﬂection of the transfer member on the supported structure, otherwise ef /1000

ef /250

Members subjected to vehicular or pedestrian trafﬁc Transfer members

1 2 3 4 5 6 7

The effective span ef is the lesser of the centre-to-centre distance between the supports and the clear span plus the member depth. For a cantilever ef is the clear projection plus half the member depth. In general, deﬂection limits should be applied to all spanning directions. This includes, but is not limited to, each individual member and the diagonal spans across each design panel. For ﬂat slabs with uniform loadings, only the column strip deﬂections in each direction need be checked. If the location of masonry partitions or other brittle ﬁnishes is known and ﬁxed, these deﬂection limits need only be applied to the length of the member supporting them. Otherwise, the more general requirements of Note 2 should be followed. Deﬂection limits given may not safeguard against ponding. For cantilevers, the deﬂection limitations given in this table apply only if the rotation at the support is included in the calculation of deﬂection. Consideration should be given by the designer to the cumulative effect of deﬂections, and this should be taken into account when selecting a deﬂection limit. When checking the deﬂections of transfer members and structures, allowance should be made in the design of the supported members and structure for the deﬂection of the supporting members. This will normally involve allowance for settling supports and may require continuous bottom reinforcement at settling columns.

live load. Such structures are generally uncracked at service loads, the total deﬂection is small and type 1 and 2 deﬂection problems are easily avoided. Where a structure supports vibrating machinery (or any other signiﬁcant dynamic load) or where a structure may be subjected to ground motion caused by earthquake, blast or adjacent road or rail trafﬁc, vibration control becomes an important design requirement. This is particularly so for slender structures, such as tall buildings or long-span beams or slabs.

44 Design for serviceability Vibration is best controlled by isolating the structure from the source of vibration. Where this is not possible, vibration may be controlled by limiting the frequency of the fundamental mode of vibration of the structure to a value that is signiﬁcantly different from the frequency of the source of vibration. When a structure is subjected only to pedestrian trafﬁc, 5 Hz is often taken as the minimum frequency of the fundamental mode of vibration of a beam or slab (Refs 19 and 20) and a method for vibration analysis is described in Ref. 20. In modern concrete structures, serviceability failures are relatively common. The tendency towards higher strength materials and the use of ultimate strength design procedures for the proportioning of structures has led to shallower, more slender elements, and consequently, an increase in deformations at service loads. As far back as 1967 (Ref. 21), the most common cause of damage in concrete structures was due to excessive slab deﬂections. If the incidence of serviceability failure is to decrease, design for serviceability must play a more signiﬁcant part in routine structural design and the structural designer must resort more often to analytical tools that are more accurate than those found in most building codes. The analytical models outlined in the remainder of this book provide designers with reliable and rational means for predicting both the short-term and time-dependent deformations in concrete structures. 3.4.2 Crack width limits In routine structural design, the calculation of crack widths is often not required. Crack control is deemed to be provided by appropriate detailing of the reinforcement and by limiting the stress in the reinforcement crossing the crack to some appropriately low value (see Section 3.7.1). The limiting steel stress depends on the maximum acceptable crack width for the structure that in turn depends on the structural requirements and the local environment. Recommended maximum crack widths are given in Table 3.2.

3.5 Maximum span-to-depth ratio – minimum thickness In the design of a reinforced concrete beam or slab, the designer is ﬁrst confronted with the problem of selecting a suitable depth or thickness of the member. In the case of ﬂoor slabs, a reasonable ﬁrst estimate is desirable since, in many cases, the self-weight of the slab is a large proportion of the total service load. Strength considerations alone may result in a slab thickness that leads to excessive deﬂection at service loads. The relatively low tensile reinforcement quantities commonly used in slabs (Ast /bd is typically in the range 0.0025–0.006) are evidence of the importance of serviceability in the selection of slab thickness. Many codes of practice specify a minimum thickness, h, or a maximum span-toeffective depth ratio, /d. The implication is that deﬂection will be acceptable if the beam or slab thickness is greater than the minimum value, and thus the deﬂection need not be calculated. For example, for normal weight concrete members containing steel reinforcement with a yield stress of fy = 500 MPa and for members that are not supporting or attached to partitions or other construction likely to be damaged by large deﬂection, ACI-318-08 (Ref. 4) speciﬁes that deﬂections need not be calculated if the thickness of a beam or one-way slab is greater than the minimum thickness given in Table 3.3

Design for serviceability

45

Table 3.2 Recommended maximum ﬁnal design crack width, w∗ Environment

Design requirement

Sheltered environment (where crack widths will not adversely affect durability)

Aesthetic requirement • where cracking could adversely affect the appearance of the structure • close in buildings • distant in buildings

0.3 0.5

•

0.7

Environment

Aggressive environment ∗c

Maximum ﬁnal crack width, w* (mm)

where cracking will not be visible and aesthetics is not important.

Durability requirement • where wide cracks could lead to corrosion of reinforcement

0.3

Durability requirement • where wide cracks could lead to corrosion of reinforcement

0.30 (when c∗ ≥ 50 mm) 0.25 (otherwise)

is the concrete cover to the nearest steel reinforcement.

Table 3.3 Minimum thickness for non-prestressed beams or one-way slabs – fy = 500 MPa (Ref. 4) Minimum thickness, h

Solid one-way slab Beam or ribbed slab

Simplysupported

One end continuous

Both ends continuous

Cantilever

/18 /14.5

/21.5 /16.5

/25 /19

/9 /7

is the span measured centre to centre of supports or the clear projection of a cantilever.

or if the thickness of a two-way ﬂat slab or ﬂat plate is greater than the value given in Table 3.4. This deemed-to-comply approach is attractive because of its simplicity and, if it always led to appropriately proportioned and serviceable slabs, it would be ideal for use in routine design. However, in some situations, the use of the minimum thicknesses in Tables 3.3 and 3.4 leads to slabs that are far thicker than they need to be. In other situations, some heavily loaded slabs with the minimum thicknesses speciﬁed in Tables 3.3 and 3.4 deﬂect excessively. Indeed, a single value for minimum thickness that does not account for the load level, the steel quantities and location, the occupancy of the structure (and therefore the desired deﬂection limit), the load duration, the quality of the concrete and the environment cannot possibly ensure deﬂection control in every situation, unless, of course, it is grossly conservative in many situations and therefore entirely unsuitable for use in structural design. Based on the work of Rangan (Ref. 22) and Gilbert (Ref. 23), the Australian Standard AS3600-2009 (Ref. 7) speciﬁes a maximum span to effective depth ratio

46 Design for serviceability Table 3.4 Minimum thickness of two-way slabs without interior beams (ﬂat slabs or ﬂat plates) – fy = 500 MPa (Ref. 4) Minimum thickness, h Without drop panels

With drop panels

Exterior panels Without edge beams n /28

Interior panels With edge beams n /31

n /31

Exterior panels Without edge beams n /31

Interior panels With edge beams n /34

n /34

n is the clear span measured face to face of supports in long span direction.

for slabs given by: ef /d = k3 k4

(/ef )1000Ec

1/3

Fd.ef

(3.1)

where ef is the lesser of the clear span plus slab thickness and the centre-to-centre distance between supports; d is the effective depth from the compressive surface of the slab to the centroid of the tensile reinforcement; is the deﬂection limit selected in design (either total or incremental deﬂection); Ec is the elastic modulus of the concrete (in MPa); Fd.ef is the effective design service load (in kPa) and is equal to 3g + q1 + 2q2 for total deﬂection and 2g + q1 + 2q2 for incremental deﬂection; g is the dead load (in kPa); q1 is the expected short-term live load (in kPa); q2 is the sustained part of the live load (in kPa); and k3 is a slab system factor given by: • • •

k3 = 1.0 for one-way slabs and two-way edge-supported slabs; k3 = 0.95 for a two-way ﬂat slab without drop panels; and k3 = 1.05 for a two-way ﬂat slab with drop panels.

The term k4 is a factor that depends on the continuity at the supports of the slab and, for a one-way slab or two-way ﬂat slab, k4 equals 1.4 for a simply-supported span, l.75 for the end span of a continuous slab and 2.1 for an interior span of a continuous slab. For a two-way edge-supported slab, k4 is given in Table 3.5. Alternative expressions for the limiting span-to-depth ratios are speciﬁed in other codes. For example, according to Eurocode 2 (Ref. 6), if the span-to-depth ratio of a member does not exceed the following limiting values, deﬂections need not be calculated for members where the maximum total deﬂection is not to exceed span/250 and where the incremental deﬂection is not to exceed span/500:

3/2 ρo ρo if ρ ≤ ρo −1 = K 11 + 1.5 fc + 3.2 fc ρ ρ d ρ 1 ρ o + f if ρ > ρo = K 11 + 1.5 fc c d ρ − ρ 12 ρo

(3.2a)

(3.2b)

Design for serviceability

47

Table 3.5 Continuity factor k4 for a rectangular slab panel supported on four sides – (Ref. 7) Edge condition

Continuity factor, k4 Ratio of long to short span (y /x )

Four edges continuous One short edge discontinuous One long edge discontinuous Two short edges discontinuous Two long edges discontinuous Two adjacent edges discontinuous Three edges discontinuous (one long edge continuous) Three edges discontinuous (one short edge continuous) Four edges discontinuous

1.0

1.25

1.5

2.0

3.60 3.40 3.40 3.20 3.20 2.95 2.70 2.70 2.25

3.10 2.90 2.65 2.80 2.50 2.50 2.30 2.10 1.90

2.80 2.70 2.40 2.60 2.00 2.25 2.20 1.90 1.70

2.50 2.40 2.10 2.40 1.60 2.00 1.95 1.60 1.50

where K depends on the structural system, with K = 1.0 for simply supported beams and one-way or two-way spanning slabs; K = 1.3 for end spans of continuous beams and one-way or two-way slabs continuous over one long side; K = 1.5 for interior spans of beams and one-way or two-way spanning slabs; K = 1.2 for ﬂat slabs supported on columns without beams (based on longer span); and K = 0.4 for a cantilever; ρo is a reference reinforcement ratio given by ρo = 0.001 fc ; ρ is the tension reinforcement ratio at mid-span required to resist the moment due to the design loads (at the support for cantilevers); ρ is the compression reinforcement ratio at mid-span (at the support for cantilevers); fc is in MPa. For ﬂanged sections where the ratio of the ﬂange width to the web width exceeds 3, the values obtained from Eqs 3.2 should be multiplied by 0.8. For beams and slabs, other than ﬂat slabs, supporting partitions likely to be damaged by excessive deﬂection and with spans exceeding 7 m, the values of /d given by Eqs 3.2 should be multiplied by 7/ef , where ef is the effective span in metres. For ﬂat slabs supporting partitions likely to be damaged by excessive deﬂection and where the longer span exceeds 8.5 m, the values of /d given by Eqs 3.2 should be multiplied by 8.5/ef . An iterative procedure is required to use Eqs 3.2. An initial estimate of the effective depth d must be made in order to calculate the reinforcement ratios ρ and ρ required to resist the design moment at the critical sections. These reinforcement ratios are in turn required in the calculation of the limiting span-to-depth ratio using Eqs 3.2. Depending on the initial estimate of d, the required reinforcement ratios may need to be recalculated, together with a revised slab depth, to ensure deﬂection control. Similarly, the use of Eq. 3.1 requires an initial estimate of slab thickness to determine the self-weight and an iteration may be required if the initial estimate is poor. On the other hand, the ACI 318-08 (Ref. 4) minimum thicknesses do not require any iteration and can be used to select an initial member thickness at the beginning of the design. Designers should be aware that the use of either the ACI 318-08 minimum thicknesses (Tables 3.3 and 3.4) or the AS3600-2009 (Ref. 7) maximum span-todepth ratio (Eq. 3.1) is inevitably conservative for most practical situations and leads

48 Design for serviceability to beam and slab thicknesses that may be considerably larger than they need to be. In contrast, the Eurocode 2 (Ref. 6) limiting span-to-depth ratios may result in beam or slab thicknesses that are unacceptably small, particularly in situations where the sustained load is a large proportion of the total load, and should not be regarded as a guarantee that deﬂections will not be excessive.

Example 3.1 The thickness of the end span of a one-way slab is to be estimated for the cases where: 1) the maximum long-term mid-span deﬂection is not to exceed span/250; and 2) the incremental deﬂection is not to exceed span/480. The span is = ef = 5.0 m; the dead load g = 2.0 kPa + self-weight; and the live load is q = 3.0 kPa. The short-term expected live load is q1 = 2.1 kPa and the sustained part of the live load q2 = 1.2 kPa. The speciﬁed concrete and reinforcement strengths are fc = 25 MPa and fy = 500 MPa; the clear concrete cover to the longitudinal reinforcement is 20 mm; and the reinforcement bar diameter is db = 12 mm.

ACI318-08 From Table 3.3, if deﬂections are not to be calculated, the minimum thickness according to ACI318-08 is h = 5000/21.5 = 230 mm, irrespective of the deﬂection requirements for the slab and irrespective of the loads to be applied to the slab.

AS3600-2009 From Table 2.1, Ec = 26700 MPa. To calculate the maximum effective span-todepth ratio using Eq. 3.1, an estimate of self-weight of the slab is required. Take self-weight = 0.23 × 24 = 5.5 kPa and the dead load is therefore g = 2.0 + 5.5 = 7.5 kPa. (i) If the maximum total deﬂection is = 5000/250 = 20 mm, then the effective design service load is Fd.ef = 3g + q1 + 2q2 = 3 × 7.5 + 2.1 + 2 × 1.2 = 27.0 kPa and, from Eq. 3.1, the maximum span to effective depth ratio is:

ef /d = 1.0 × 1.75

(20/5000) × 1000 × 26700 27.0

1/3 = 27.7

The minimum effective depth according to AS 3600-2009 is therefore d = 5000/27.7 = 181 mm and the minimum slab thickness is h = d + db /2 + cover = 181 + 6 + 20 = 207 mm.

Design for serviceability

49

(ii) If the incremental deﬂection is = 5000/480 = 10.4 mm, then the effective design service load is Fd.ef = 2g + q1 + 2q2 = 2 × 7.5 + 2.1 + 2 × 1.2 = 19.5 kPa and, from Eq. 3.1, the maximum span to effective depth ratio is:

ef /d = 1.0 × 1.75

(10.4/5000) × 1000 × 26700 19.5

1/3 = 24.8

The minimum effective depth according to AS 3600-2009 is therefore d = 5000/24.8 = 201 mm and the minimum slab thickness is h = d + db /2 + cover = 201 + 6 + 20 = 227 mm.

Eurocode 2 If the design moment at mid-span is w∗ 2 /12, where w∗ is the factored design load for the strength limit state, and if after several iterations the initial estimate of d is 150 mm, the reinforcement ratio required to resist the design moment is ρ = 0.0035 and ρ = 0. The reference reinforcement ratio is ρo = 0.001 fc = 0.005 and the factor K = 1.3. From Eq. 3.2a:

3/2 √ √ 0.005 0.005 = 1.3 11 + 1.5 25 = 34.1 + 3.2 25 −1 d 0.0035 0.0035 The minimum effective depth according to Eurocode 2 is therefore d = 5000/34.1 = 147 mm and the minimum slab thickness is h = d + db /2 + cover = 147 + 6 + 20 = 173 mm. Clearly, in this example, the minimum slab thickness obtained using Eq. 3.2a from Eurocode 2 is signiﬁcantly smaller than the value obtained using either the ACI 318-08 minimum thickness provisions or the maximum span to depth ratio speciﬁed in AS 3600-2009.

3.6 Deﬂection control by simpliﬁed calculation 3.6.1 Calculation of deformation If the axial strain and curvature are known at regular intervals along a member, it is a relatively simple task to determine the deformation of that member. Consider the statically determinate member subjected to the axial and transverse loads shown in Fig. 3.1. The axial deformation of the member eAB (either elongation or shortening) is obtained by integrating the axial strain at the centroid of the member, εa (z), over the length of the member. That is: eAB =

0

εa (z) dz

where z is measured along the member, as shown.

(3.3)

50 Design for serviceability Load B

A C /2

/2

z

(a) Original geometry vC qA

A, A′

eAB B, B′

qB

C′ (b) Deformed shape

Figure 3.1 Deformation of a statically determinate member.

Provided that deﬂections are small and that simple beam theory is applicable, the slope θ and deﬂection v at any point z along the member are obtained by integrating the curvature κ(z) along the member as follows: θ=

κ(z) dz

(3.4)

v=

κ(z) dz dz

(3.5)

Eqs 3.4 and 3.5 are quite general and apply to both elastic and inelastic material behaviour. If the axial strain and curvature are calculated at any time after loading at a preselected number of points along the member shown in Fig 3.1 and if a reasonable variation of strain and curvature is assumed between adjacent points, it is a simple matter of geometry to determine the deformation of the member. For convenience, some simple equations are given below for the determination of the deformation of a single span and of a cantilever. If the axial strain εa and the curvature κ are known at the mid-span and at each end of the member shown in Fig 3.1 (i.e. at supports A and B and at point C), the axial deformation eAB , the slope at each support θA and θB and the deﬂection at mid-span vC are given by Eqs 3.6 and 3.7. For a linear variation of strain and curvature: eAB =

(εaA + 2 εaC + εaB ) 4

2 (κA + 4 κC + κB ) 48 θA = (5 κA + 6 κC + κB ) 24 θB = − (κA + 6 κC + 5 κB ) 24

vC =

(3.6a) (3.6b) (3.6c) (3.6d)

Design for serviceability

51

For a parabolic variation of strain and curvature: eAB =

(εaA + 4 εaC + εaB ) 6

(3.7a)

vC =

2 (κA + 10 κC + κB ) 96

(3.7b)

θA =

(κA + 2 κC ) 6

(3.7c)

θB = −

(2κC + κB ) 6

(3.7d)

In addition to the simple span shown in Fig. 3.1, Eqs 3.6 and 3.7 also apply to any member in a statically indeterminate frame, provided the strain and curvature at each support and at mid-span are known. Consider the ﬁxed-end cantilever shown in Fig. 3.2. If the curvatures at A, B and C are known, then the slope and deﬂection at the free end of the member are given by Eqs 3.8 and 3.9. For a linear variation of curvature: θC = − (κA + 2κB + κC ) 4 vC = −

(3.8a)

2 (5κA + 6 κB + κC ) 24

(3.8b)

For a parabolic variation of curvature: θC = − (κA + 4κB + κC ) 6 vC = −

(3.9a)

2 (κA + 2κB ) 6

(3.9b)

If the curvatures at the ﬁxed and free ends of the cantilever only are known (i.e. at A and C), then the slope and deﬂection at the free end C are given by Eqs 3.10 and 3.11.

A

B

C vC qC

Figure 3.2 Deformation of a ﬁxed-end cantilever.

52 Design for serviceability For a linear variation of curvature: θC = −

(κA + κC ) 2

(3.10a)

vC = −

2 (2κA + κC ) 6

(3.10b)

For a parabolic variation of curvature (typical of what occurs in a uniformly loaded cantilever): θC = −

(κA + 2κC ) 3

(3.11a)

vC = −

2 (κA + κC ) 4

(3.11b)

3.6.2 Load versus deﬂection response of a reinforced concrete member The short-term or instantaneous deformation of a cracked reinforced concrete crosssection subjected to combined bending and axial force can be readily determined using simple modular ratio theory (Section 3.6.3). After cracking, the properties of both the fully-cracked section and the uncracked section are often combined empirically to model tension stiffening and to approximate the average properties of the cracked region. Consider the load-deﬂection response of a simply-supported, singly reinforced concrete beam or one-way slab shown in Fig. 3.3. At loads less than the cracking load, Pcr , the member is uncracked and behaves homogeneously and elastically. The slope of the load-deﬂection plot (OA in Fig. 3.3) is proportional to the second moment of area of the uncracked transformed section, Iuncr . The member ﬁrst cracks at Pcr when the extreme ﬁbre tensile stress in the concrete at the section of maximum moment reaches the ﬂexural tensile strength of the concrete, fct.f . There is a sudden change in the local stiffness at, and immediately adjacent to, this ﬁrst crack. At the section containing the crack, the ﬂexural stiffness drops signiﬁcantly, but the rest of the member remains uncracked. As load increases, more cracks form and the average ﬂexural stiffness of the entire member decreases. If the tensile concrete in the cracked regions of the beam carried no stress, the load-deﬂection relationship would follow the dashed line ACD. If the average extreme ﬁbre tensile stress in the concrete remained at fct.f after cracking, the load-deﬂection relationship would follow the dashed line AE. In reality, the actual response lies between these extremes and is shown in Fig. 3.3 as the solid line AB. The difference between the actual response and the zero tension response is the tension stiffening effect (that reduces the instantaneous deﬂection by δ as shown). Tension stiffening is the contribution of the intact tensile concrete between the cracks to the post-cracking stiffness of the member. At each crack, the tensile concrete carries no stress, but as the distance from the crack increases, the tensile stress in the concrete increases due to the bond between the concrete and the tensile reinforcement. As the load increases, the average tensile stress in the concrete reduces as more cracks develop and, when the crack pattern is fully developed and the number of cracks has stabilised, the actual response becomes approximately parallel to the no tension response (OD in Fig. 3.3). For slabs containing small quantities of tensile reinforcement

Design for serviceability Deflection assuming no cracking

Load

Tension stiffening, dD E

B

53

D

Actual response

Pservice

Pcr

Concrete carries no tension anywhere A

C

Concrete carries no tension in the cracked regions Deflection O

Figure 3.3 Typical load versus deﬂection relationship.

(typically in ﬂoor slabs Ast /bd < 0.005), tension stiffening may be responsible for more than 50 per cent of the stiffness of the cracked member at service loads and δ remains signiﬁcant up to and beyond the point where the steel yields and the ultimate load is approached. Figure 3.4a shows an elevation of a singly reinforced concrete ﬂexural member subjected to a uniform bending moment M of sufﬁcient magnitude to establish the primary ﬂexural cracks. The variation of stress in the tensile reinforcement along the member is shown in Fig. 3.4b and the variation of tensile stress in the concrete at the steel level is shown in Fig. 3.4c. Over a gauge length containing several cracks, the average concrete tensile stress σc.avg at typical in-service levels of applied moment is a signiﬁcant percentage of the tensile strength of the concrete. The keys to predicting the instantaneous deﬂection are ﬁrst to evaluate the load required to cause ﬁrst cracking or, more precisely, the moment to cause ﬁrst cracking at the critical cross-section, and secondly to model tension stiffening accurately. Both of these tasks are not straightforward. Restraint to shrinkage provided by the bonded reinforcement and restraint to shrinkage at the member’s ends can cause signiﬁcant tension in the concrete in the ﬁrst few days after casting. Cracking may therefore occur at loads far less than that required to produce an extreme ﬁbre tensile stress equal to the modulus of rupture fct.f in a member without shrinkage. One commonly used approach for modelling tension stiffening in deﬂection calculations involves determining an average effective second moment of area (Ief ) for a cracked member. For a prismatic member, the effective second moment of area after cracking is less than the second moment of area of the uncracked transformed section (Iuncr ) and greater than the second moment of area of the fully-cracked crosssection (Icr ). Several different empirical equations are available for Ief , including the well-known equation developed by Branson (Ref. 17) that is included in ACI 318-08. A modiﬁed and signiﬁcantly more realistic version of Branson’s equation is speciﬁed in AS3600-2009. Another model for Ief was recently proposed by Bischoff (Ref. 24) and may be derived from the method speciﬁed in Eurocode 2 for

54 Design for serviceability Primary cracks M

M

ho Reinforcement (a) Elevation

sst.max

(b) Stress in tensile reinforcement

sc.avg (c) Tensile stress in concrete at steel level

Figure 3.4 Stress distributions at the steel level in a cracked reinforced concrete member.

the calculation of deﬂection. These approaches are presented and reviewed in the following sub-sections. 3.6.3 Modular ratio theory The second moment of area of a reinforced concrete cross-section is conventionally calculated using linear elastic analysis with the following assumptions: (i) plane sections remain plane (i.e. the strain distribution is linear); (ii) perfect bond exists between the reinforcement and the concrete; and (iii) the stress-strain relationships for concrete and steel are linear and elastic. The steel reinforcement is transformed into an equivalent area of concrete by multiplying the reinforcement area by the modular ratio n (where n = Es /Ec ) and the properties of the cross-section are determined using the principles of mechanics of solids. After cracking, the concrete in tension is assumed to carry no stress. This simple procedure is often called modular ratio theory and it is used to calculate the second moment of area of the section before and after cracking. In itself, it does not account for tension stiffening and does not include the time-dependent deformations caused by creep and shrinkage. Figure 3.5 shows the strains, stresses and resultant forces on a cracked, singly reinforced, rectangular cross-section subjected to an applied moment M. With regard to the stresses and deformations, there are two unknowns – the top ﬁbre compressive strain εtop and the depth to the neutral axis dn = kd. The depth to the neutral axis may be determined by equating the resultant compressive and tensile forces (i.e. by enforcing the requirement of equilibrium of longitudinal forces): C=T 0.5 σtop b kd = σst Ast

Design for serviceability b

kd/3 etop

stop

dn= kd

D

d N

55

A

C = ½stop b kd f = d(1−k/3)

M (1–k)d Ast

(a) Cross-section

est

(b) Strains

T = sst Ast

sst

(c) Stresses

(d) Forces

Figure 3.5 Strains, stresses and forces on a cracked section in bending.

and, assuming linear-elastic stress-strain laws for the reinforcement and the compressive concrete, this becomes: 0.5k =

εst Es Ast εst σst Ast = = nρ εtop Ec bd εtop σtop bd

(3.12)

where ρ is the tensile reinforcement ratio, Ast /bd. Compatibility requires that the strain diagram is linear and therefore: (1 − k)d 1 − k εst = = εtop kd k

(3.13)

Substituting Eq. 3.13 into Eq. 3.12 gives: 0.5k =

1−k nρ k

and solving this quadratic equation for k gives: k = (nρ)2 + 2nρ − nρ

(3.14)

It should be noted that k (and hence the depth to the neutral axis kd) depends only on the modular ratio n and the reinforcement ratio ρ and is independent of the applied moment M. The depth to the neutral axis remains constant after cracking as the moment increases, until either the concrete compressive stress distribution becomes curvilinear or the reinforcing steel yields. With k determined from Eq. 3.14, the top ﬁbre concrete stress σtop and the steel stress σst may be found from the moment equilibrium equation: M = C f = T f = ½σtop b kd2 (1 − k/3) = σst Ast d(1 − k/3) and hence σtop =

2M M and σst = Ast d(1 − k/3) b kd 2 (1 − k/3)

(3.15)

56 Design for serviceability Clearly, the stresses in both the concrete and the steel are linear functions of the applied moment M. With the stress and strain distributions established, the ﬂexural rigidity of the cracked section (Ec Icr ) may be obtained from the curvature (i.e. the slope of the strain diagram) as follows: εtop σtop M 2M = = = Ec Icr kd Ec kd Ec bk2 d 3 (1 − k/3)

(3.16)

From Eq. 3.16, the second moment of area of the cracked section is: Icr = ½ b d 3 k2 (1 − k/3)

(3.17)

For convenience, values of the neutral axis parameter k and the cracked second moment of area Icr of singly reinforced rectangular sections are given in Table 3.6. Table 3.6 Neutral axis depth (kd) and second moment of area (Icr = λbd3 ) for singly reinforced rectangular sections (n = Es /Ec ) ρ = Ast /bd

0.002 0.0025 0.003 0.0035 0.004 0.0045 0.005 0.0055 0.006 0.0065 0.007 0.0075 0.008 0.0085 0.009 0.0095 0.010 0.011 0.012 0.013 0.014 0.015 0.016 0.017 0.018 0.019 0.020

n=4

n=5

n=6

n=7

n=8

n=9

n = 10

k

λ

k

λ

k

λ

k

λ

k

λ

k

λ

k

λ

0.119 0.132 0.143 0.154 0.164 0.173 0.181 0.189 0.196 0.204 0.210 0.217 0.223 0.229 0.235 0.240 0.246 0.256 0.266 0.275 0.283 0.292 0.299 0.307 0.314 0.321 0.328

0.0068 0.0083 0.0098 0.0112 0.0127 0.0140 0.0154 0.0167 0.0180 0.0193 0.0206 0.0218 0.0230 0.0242 0.0254 0.0266 0.0277 0.0299 0.0321 0.0343 0.0363 0.0384 0.0404 0.0423 0.0442 0.0461 0.0479

0.132 0.146 0.159 0.170 0.181 0.191 0.200 0.209 0.217 0.225 0.232 0.239 0.246 0.252 0.258 0.264 0.270 0.281 0.292 0.301 0.311 0.319 0.328 0.336 0.344 0.351 0.358

0.0083 0.0102 0.0119 0.0137 0.0154 0.0170 0.0187 0.0202 0.0218 0.0233 0.0248 0.0263 0.0277 0.0291 0.0305 0.0319 0.0332 0.0358 0.0384 0.0408 0.0433 0.0456 0.0479 0.0501 0.0523 0.0544 0.0565

0.143 0.159 0.173 0.185 0.196 0.207 0.217 0.226 0.235 0.243 0.251 0.258 0.266 0.272 0.279 0.285 0.292 0.303 0.314 0.325 0.334 0.344 0.353 0.361 0.369 0.377 0.384

0.0098 0.0119 0.0140 0.0161 0.0180 0.0199 0.0218 0.0236 0.0254 0.0271 0.0288 0.0305 0.0321 0.0337 0.0353 0.0369 0.0384 0.0413 0.0442 0.0470 0.0497 0.0523 0.0548 0.0573 0.0597 0.0621 0.0644

0.154 0.170 0.185 0.198 0.210 0.221 0.232 0.242 0.251 0.260 0.268 0.276 0.283 0.291 0.298 0.304 0.311 0.323 0.334 0.345 0.355 0.365 0.374 0.383 0.392 0.400 0.407

0.0112 0.0137 0.0161 0.0183 0.0206 0.0227 0.0248 0.0268 0.0288 0.0308 0.0327 0.0345 0.0363 0.0381 0.0399 0.0416 0.0433 0.0465 0.0497 0.0527 0.0557 0.0585 0.0613 0.0640 0.0667 0.0692 0.0717

0.164 0.181 0.196 0.210 0.223 0.235 0.246 0.256 0.266 0.275 0.283 0.292 0.299 0.307 0.314 0.321 0.328 0.341 0.353 0.364 0.374 0.384 0.394 0.403 0.412 0.420 0.428

0.0127 0.0154 0.0180 0.0206 0.0230 0.0254 0.0277 0.0299 0.0321 0.0343 0.0363 0.0384 0.0404 0.0423 0.0442 0.0461 0.0479 0.0514 0.0548 0.0581 0.0613 0.0644 0.0674 0.0703 0.0731 0.0758 0.0785

0.173 0.191 0.207 0.221 0.235 0.247 0.258 0.269 0.279 0.289 0.298 0.306 0.314 0.322 0.330 0.337 0.344 0.357 0.369 0.381 0.392 0.402 0.412 0.421 0.430 0.438 0.446

0.0140 0.0170 0.0199 0.0227 0.0254 0.0280 0.0305 0.0329 0.0353 0.0376 0.0399 0.0421 0.0442 0.0463 0.0483 0.0503 0.0523 0.0561 0.0597 0.0633 0.0667 0.0699 0.0731 0.0762 0.0791 0.0820 0.0848

0.181 0.200 0.217 0.232 0.246 0.258 0.270 0.281 0.292 0.301 0.311 0.319 0.328 0.336 0.344 0.351 0.358 0.372 0.384 0.396 0.407 0.418 0.428 0.437 0.446 0.455 0.463

0.0154 0.0187 0.0218 0.0248 0.0277 0.0305 0.0332 0.0358 0.0384 0.0408 0.0433 0.0456 0.0479 0.0501 0.0523 0.0544 0.0565 0.0605 0.0644 0.0681 0.0717 0.0752 0.0785 0.0817 0.0848 0.0878 0.0908

Design for serviceability

57

3.6.4 AS 3600-2009 and ACI 318-08 3.6.4.1 Instantaneous deﬂection According to AS 3600-2009, the instantaneous or short-term deﬂection of a beam may be calculated using the mean value of the elastic modulus of concrete at the time of ﬁrst loading, Ec , together with the effective second moment of area of the span Ief . The effective second moment of area involves an empirical adjustment of the second moment of area of a cracked member to account for tension stiffening. For a given cross-section, Ief is calculated using Branson’s formula (Ref. 17): Ief = Icr + (Iuncr − Icr )(Mcr /Ms∗ )3 ≤ Ief ,max

(3.18)

where Icr is the second moment of area of the fully-cracked section (calculated using modular ratio theory); Iuncr is the second moment of area of the uncracked crosssection about its centroidal axis; Ms∗ is the maximum bending moment at the section, based on the short-term serviceability design load or the construction load; Mcr is the cracking moment given by: Mcr = Z(fct.f − σcs + P/A) + Pe ≥ 0.0

(3.19)

where Z is the section modulus of the uncracked section, referred to the extreme ﬁbre at which cracking occurs; fct.f is the characteristic ﬂexural tensile strength of concrete speciﬁed as fct.f = 0.6 fc ; P is the effective prestressing force (if any); e is the eccentricity of prestress measured to the centroidal axis of the section; A is the area of the uncracked cross-section; and σcs is the maximum shrinkage-induced tensile stress on the uncracked section at the extreme ﬁbre at which cracking occurs. In the absence of more reﬁned calculation, σcs may be taken as:

2.5ρw − 0.8ρcw ∗ σcs = (3.20) Es εsh 1 + 50ρw where ρw is the web reinforcement ratio for the tensile steel (Ast + Apt )/bw d; ρcw is the web reinforcement ratio for the compressive steel, if any (Asc /bw d); Ast is the area on non-prestressed tensile reinforcement; Apt is the area of prestressing steel in the tensile zone; Asc is the area of non-prestressed compressive reinforcement; Es is ∗ is the ﬁnal design shrinkage strain the elastic modulus of the steel in MPa; and εsh (after 30 years). For non-prestressed members, the maximum value of Ief at any crosssection in Eq. 3.18 is Ief ,max = Iuncr when ρ = Ast /bd ≥ 0.005 and Ief ,max = 0.6Iuncr when ρ < 0.005. For a simple-supported beam or slab, the value of Ief for the member is determined from the value of Ief at mid-span. For interior spans of continuous beams or slabs, Ief is half of the value of Ief at mid-span plus one quarter of the value of Ief at each support, while for end spans of continuous beams or slabs, Ief is half the mid-span value plus half the value at the continuous support. For a cantilever, Ief is the value of Ief at the support. The term σcs is introduced into Eq. 3.19 to allow for the reduction in the cracking moment that inevitably occurs because of the restraint to shrinkage provided by the bonded tensile reinforcement. Shrinkage-induced tension often causes extensive

58 Design for serviceability time-dependent cracking, particularly in lightly loaded members. This time-dependent cracking may occur weeks and months after the member is ﬁrst loaded and must be accounted for if a meaningful estimate of deﬂection is required. Eq. 3.20 is based on the expression originally proposed by Gilbert (Ref. 26) for singly reinforced rectangular sections, where conservative values were assumed for the elastic modulus and the creep coefﬁcient of concrete and about 70 per cent of the ﬁnal shrinkage was considered in the calculation of Mcr . The expression was modiﬁed to accommodate the inclusion of compressive reinforcement (Ref. 27). The calculation of σcs for more general crosssections is discussed in detail in Ref. 28. Where appropriate, the additional tension that may arise due to restraint to shrinkage provided by the supports of a beam or slab should also be taken into account. The allowance for shrinkage-induced tension is particularly important in the case of lightly reinforced members (including slabs) where the tension induced by the full service moment alone might not be enough to cause cracking. In such cases, failure to account for shrinkage may lead to deﬂection calculations in which cracking is not adequately taken into account and this may lead to gross underestimates of the actual deﬂection. For heavily reinforced sections, the problem is not as signiﬁcant, because the service loads are usually well in excess of the cracking load and tension stiffening is not as signiﬁcant. ACI 318-08 also speciﬁes Eq. 3.18, except that the gross second moment of area, Ig , is used rather than Iuncr and, with Mcr given by Z (0.62 fc ), it does not include any allowance for shrinkage-induced tension or the loss of stiffness caused by cracking due to early shrinkage. For many slabs, cracking will occur within weeks of casting due to early drying shrinkage and temperature changes, often well before the slab is exposed to its full service loads. In a recent comparison of the instantaneous deﬂection predicted by ACI 318-08 and the measured deﬂections of lightly reinforced concrete slabs (Ref. 18), ACI 318-08 signiﬁcantly underestimated the instantaneous deﬂection after cracking of every slab and, for the very lightly reinforced slabs (ρ < 0.003), the deﬂection was grossly underestimated. In addition, ACI 318 does not model the abrupt change in direction of the moment-deﬂection response at ﬁrst cracking and does not predict the correct shape of the moment-deﬂection plot after cracking (Ref. 18). 3.6.4.2 Time-dependent deﬂection For the calculation of long-term deﬂection, one of two approaches is speciﬁed in AS 3600-2009. For reinforced or prestressed beams, the creep and shrinkage deﬂections can be calculated separately (using the material data speciﬁed in the standard and the principles of mechanics). Alternatively, for reinforced concrete beams and slabs, the additional long-term deﬂection caused by creep and shrinkage may be crudely approximated by multiplying the short-term or immediate deﬂection caused by the sustained load by a multiplier kcs given by: kcs = [2 − 1.2(Asc /Ast )] ≥ 0.8

(3.21)

where Asc is the area of steel in the compressive zone of the cracked section between the neutral axis and the extreme compressive ﬁbre and the ratio Asc /Ast is taken at mid-span for a simple or continuous span and at the support for a cantilever.

Design for serviceability

59

ACI 318-08 also speciﬁes that unless a more comprehensive analysis is undertaken the additional long-term deﬂection resulting from the creep and shrinkage of ﬂexural members may be determined by multiplying the immediate deﬂection caused by the sustained load by a multiplier λ given by: λ =

ξ (1 + 50Asc /bd)

(3.22)

where Asc /bd is taken at mid-span for a simple or continuous span and at the support for a cantilever; and the time-dependent factor ξ depends on the duration of loads, with ξ = 2.0 for 5 years or more; ξ = 1.4 for 1 year; ξ = 1.2 for 6 months; and ξ = 1.0 for 3 months. The use of a deﬂection multiplier (kcs or λ ) to calculate time-dependent deﬂections is simple and convenient and, provided the section is initially cracked under shortterm loads, it may provide a ‘ball-park’ estimate of the ﬁnal deﬂection. However, to calculate the shrinkage-induced deﬂection by multiplying the load-induced short-term deﬂection by a long-term deﬂection multiplier is fundamentally incorrect. Shrinkage can cause signiﬁcant deﬂection even in unloaded members. The approach ignores many of the factors that inﬂuence the ﬁnal deﬂection, including the creep and shrinkage characteristics of the concrete, the environment and the age at ﬁrst loading. At best, it must be seen as providing a very approximate estimate. At worst, it is misleading and not worth the time involved in making the calculation. In addition, when using the ACI 318-08 multiplier, no account is taken of the loss of stiffness caused by shrinkageinduced cracking at any stage of the calculation procedure and, in the case of slabs, this may be very signiﬁcant. It is, however, not too much more complicated to calculate long-term creep and shrinkage deﬂections separately and this is the subject of much of the rest of this book. A recently proposed simpliﬁed method for deﬂection calculation that does calculate the creep and shrinkage deﬂections separately (and more accurately) is outlined in Section 3.6.6.

Example 3.2 The ﬁnal long-term deﬂection (vC )max at the mid-point C in the end span of a continuous one-way slab is to be calculated using the simpliﬁed procedures in AS 3600-2009 and ACI 318-08. The slab is 180 mm thick. The span is = ef = 5.0 m, the dead load g = 2.0 kPa + self-weight = 6.4 kPa, and the live load is q = 3.0 kPa. The short-term expected live load is q1 = 2.1 kPa and the sustained part of the live load is q2 = 1.2 kPa. The deﬂection requirement is that (vC )max ≤ ef /250 = 20 mm. = 0.6 f = 3.0 MPa The concrete and steel strengths are fc = 25 MPa, fct.f c and fy = 500 MPa. The elastic moduli for concrete and steel are Ec = 26,700 MPa and Es = 200,000 MPa, and the modular ratio is therefore n = Es /Ec = 7.5. The ∗ = 0.0007 and the clear concrete ﬁnal long-term shrinkage strain is taken to be εsh cover to the reinforcement is 20 mm.

60 Design for serviceability The bottom longitudinal reinforcement throughout the span consists of 12 mm diameter bars at 250 mm centres (Ast = 440 mm2 /m at d = 154 mm) and the top reinforcement at the interior support consists of 12 mm bars at 200 mm centres (Ast = 550 mm2 /m at d = 154 mm), as shown in Fig. 3.6. The reinforcement has been designed to provide adequate strength. Also shown in Fig. 3.6 is the bending moment diagram under the maximum uniformly distributed service load, wmax = g + q1 = 8.5 kPa. wmax = 8.5 kN/m2 N12@200 mm A A

C N12@250 mm B `=5m

(a) Elevation of end span

C −

D = 180 mm

+

B MB = −22.5 kNm/m

MC = +15.4 kNm/m

(b) Load and bending moment diagrams

Figure 3.6 Slab elevation, load and bending moment diagrams (Example 3.2).

AS3600-2009 Section at mid-span C The maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m. With Ast = 440 mm2 /m and d = 154 mm, the reinforcement ratio ρ = Ast /bd = 0.00286 and nρ = 0.0214, the centroidal axis of the uncracked transformed cross-section is 91.0 mm below the top surface and the second moment of area of the uncracked transformed section about its centroidal axis is Iuncr = 498 × 106 mm4 /m. The depth to the neutral axis for the cracked section is calculated using Eq. 3.14: k=

(0.0214)2 + 2 × 0.0214 − 0.0214 = 0.187

and therefore dn = kd = 28.7 mm. The second moment of area of the fullycracked transformed section, Icr , is next obtained from Eq. 3.17 as: Icr = ½b d 3 k2 (1 − k/3) = 59.6 × 106 mm4 /m. The bottom ﬁbre section modulus of the uncracked section is Z = Iuncr /yb = 5.59 × 106 mm3 /m. From Eq. 3.20, the shrinkage-induced tension in the bottom ﬁbre of the uncracked section is: σcs =

2.5 × 0.00286 × 2 × 105 × 0.0007 = 0.875 MPa 1 + 50 × 0.00286

Design for serviceability and the time-dependent cracking moment is obtained from Eq. 3.19 is: Mcr = 5.59 × 106 (3.00 − 0.875) × 10−6 = 11.9 kNm/m From Eq. 3.18, the effective second moment of area at mid-span is: (Ief )C = 59.6 × 106 + (498 × 106 − 59.6 × 106 )(11.9/15.4)3 = 261 × 106 mm4 /m Section at continuous B The maximum in-service moment at support B is Ms∗ = −22.5 kNm/m. At this critical section, Ast = 550 mm2 /m, d = 154 mm, ρ = 0.00357 and nρ = 0.0268. The section properties calculated as above are Iuncr = 500 × 106 mm4 /m, k = 0.206, and Icr = 72.2 × 106 mm4 /m. From Eq. 3.20, σcs = 1.06 MPa and the cracking moment is Mcr = 10.9 kNm/m. From Eq. 3.18, (Ief )B = 121 × 106 mm4 /m. For entire span The average effective second moment of area for the entire end span is taken as the average of the values at mid-span and at the continuous support. That is: Ief = 0.5 × ((Ief )C + (Ief )B ) = 0.5 × (261 × 106 + 121 × 106 ) = 191 × 106 mm4 /m Instantaneous deﬂection Assuming a uniform average rigidity for the span of Ec Ief , the instantaneous curvatures at the sections at mid-span and at the continuous support under the full service load after the effects of all cracking have been included are: (κi )C =

Ms∗ 15.4 × 106 = = 3.02 × 10−6 mm−1 Ec Ief 26,700 × 191 × 106

and (κi )B = −4.41 × 10−6 mm−1 The instantaneous deﬂection at mid-span due to the full service load after accounting for all load and shrinkage-induced cracking is obtained from Eq. 3.7b as: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 3.02 × 10−6 − 4.41 × 10−6 ) = 6.7 mm 96

61

62 Design for serviceability Time-dependent deﬂection In this example, the sustained load is wsus = g + q2 = 7.6 kPa. The instantaneous deﬂection due to the sustained loads is therefore: (vC )i.sus = (vC )i.max (wsus /wmax ) = 6.0 mm With no compressive reinforcement, the time-dependent deﬂection multiplication factor given by Eq. 3.21 is kcs = 2.0 and the time-dependent deﬂection at mid-span is: (vC )time = kcs (vC )i.sus = 2.0 × 6.0 = 12.0 mm The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is the sum of the instantaneous deﬂection due to the maximum service load and the time-dependent deﬂection due to creep and shrinkage and is given by: (vC )max = (vC )i.max + (vC )time = 6.7 + 12.0 = 18.7 mm = span/267 Discussion According to AS3600-2009, this slab will deﬂect a little less than the maximum deﬂection limit of span/250 and so the slab is just serviceable. A slightly thinner slab may be possible with the inclusion of some compressive reinforcement in the positive moment region. It is of interest to note that the deemed to comply maximum span-to-depth ratio in AS 3600-2009 is more conservative requiring minimum slab thickness of 207 mm, if deﬂections were not to be checked by calculation (see Example 3.1).

ACI318-08 Section at mid-span C The second moment of area of the gross cross-section is Ig = 486 × 106 mm4 /m. As calculated previously, with Ast = 440 mm2 /m and d = 154 mm, the second moment of area of the fully-cracked transformed section is Icr = 59.6 × 106 mm4 /m. The bottom ﬁbre section modulus of the gross section is Z = Ig /yb = 5.4 × 106 mm3 /m and the cracking moment is Mcr = Z(0.62 fc ) = √ 5.4 × 106 (0.62 25) × 10−6 = 16.7 kNm/m. According to ACI 318-08, with Ms∗ = 15.4 kNm/m, the slab will not crack in the positive moment region at any stage throughout its life and (Ief )C = Ig = 486 × 106 mm4 /m – a conclusion that experience would suggest is unsupportable. Section at continuous support B With Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d= 154 mm, Icr = 72.2×106 mm4 /m and Mcr = 16.7 kNm/m, Eq. 3.18 gives (Ief )B = 243 × 106 mm4 /m.

Design for serviceability For entire span According to ACI 318-08, the average effective second moment of area for the entire span may be taken as either the value at mid-span or the average of the values obtained at the positive and negative moment regions. For this typical example, taking the value at mid-span would be unconservative (and unwise), as the effects of any cracking would be completely ignored. Assuming that Ief is the average of the values at mid-span and at the continuous support gives Ief = 364 × 106 mm4 /m. Instantaneous deﬂection Assuming a uniform average rigidity for the span of Ec Ief , the instantaneous curvatures at the section at mid-span and at the continuous support under the full service load are (κi )C = 1.58 × 10−6 mm−1 and (κi )B = −2.31 × 10−6 mm−1 . From Eq. 3.7b, the instantaneous deﬂection at mid-span due to the full service load is: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 1.58 × 10−6 − 2.31 × 10−6 ) = 3.5 mm 96

Time-dependent deﬂection In this example, (vC )i.sus = (vC )i.max (wsus /wmax ) = 3.1 mm and with no compressive reinforcement, the time-dependent deﬂection multiplication factor given by Eq. 3.22 for a load duration of more than 5 years is λ = 2.0 and the time-dependent deﬂection at mid-span is: (vC )time = λ (vC )i.sus = 2.0 × 3.1 = 6.2 mm The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.max + (vC )time = 3.5 + 6.2 = 9.7 mm = span/515 Discussion According to ACI 318-08, the maximum ﬁnal long-term deﬂection of this 180 mm thick slab is less than half of that calculated by AS 3600-2009 and a signiﬁcantly thinner slab would be possible if the maximum ﬁnal deﬂection were to be limited to span/250. Clearly, the loss of stiffness due to shrinkageinduced cracking is ignored by ACI 318-08. Comparison of the ACI 318-08 predictions with the observed deﬂections in real slabs conﬁrms that often this method grossly underestimates deﬂection.

63

64 Design for serviceability By contrast, the minimum thickness speciﬁed for this slab in ACI 318-08 is 230 mm (see Example 3.1) and the selection of a slab thickness that met this requirement would be a very conservative design decision.

3.6.5 Eurocode 2 3.6.5.1 Instantaneous curvature An alternative approach for the calculation of deﬂection in a cracked reinforced concrete member is speciﬁed in Eurocode 2 (Ref. 6). This approach involves the calculation of the curvature at particular cross-sections and then twice integrating the curvatures along the member to obtain its deﬂection. The instantaneous curvature at a section after cracking, κ, is calculated as a weighted average of the values calculated on a fully-cracked section (κcr ) and on an uncracked section (κuncr ) as follows: κ = ζ κ cr + (1 − ζ )κuncr

(3.23)

where ζ is a distribution coefﬁcient that accounts for the moment level and the degree of cracking and, for members containing deformed bars, is given by: ζ = 1−β

σsr σs

2 (3.24a)

where β is a coefﬁcient to account for the effects of duration of loading or repeated loading on the average deformation and equals 1.0 for a single, short-term load and 0.5 for sustained loading or for many cycles of repeated loading; σsr is the stress in the tensile reinforcement at the load causing ﬁrst cracking that is calculated by ignoring concrete in tension and ignoring any shrinkage-induced tension; σs is stress in the reinforcement at the load under consideration that is calculated by ignoring concrete in tension; κcr is the curvature at the section calculated by ignoring concrete in tension; and κuncr is the curvature on the uncracked transformed section. If the compressive concrete and the reinforcement are both linear and elastic, the ratio σsr /σs in Eq. 3.24a can be replaced by Mcr /Ms∗ and therefore: ζ = 1−β

Mcr Ms∗

2 (3.24b)

The cracking moment Mcr is the moment required to produce an extreme ﬁbre tensile stress equal to the mean uniaxial tensile strength of concrete, fctm . For a reinforced concrete section in pure bending Mcr = Zfctm , where Z is the section modulus of the uncracked section, referred to the extreme ﬁbre at which cracking occurs, and fctm = 0.3(fc )2/3 when fc ≤ 50 MPa. The introduction of β = 0.5 in Eqs 3.24 for long-term deﬂection calculations is tantamount to reducing the cracking moment by about 30 per cent and is a crude way of accounting for shrinkage-induced tension and time-dependent cracking.

Design for serviceability

65

3.6.5.2 Time-dependent curvature For sustained loads, Eurocode 2 speciﬁes that the total load-induced deformation including creep may be calculated by using an effective modulus for concrete, Ee , given by: Ee =

Ec 1 + ϕ(∞, τ )

(3.25)

where ϕ(∞, τ ) is the creep coefﬁcient at time inﬁnity due to a load ﬁrst applied at time τ . The shrinkage-induced curvature κsh is obtained from the following expression: κsh = εsh ne

S I

(3.26)

where εsh is the free shrinkage strain; ne is the effective modular ratio (Es /Ee ); S is the ﬁrst moment of area of the reinforcement about the centroid of the section; and I is the second moment of area of the section. S and I and the corresponding curvatures should be calculated for both the uncracked condition and for the fully-cracked condition, and the ﬁnal average shrinkage-induced curvature in the cracked region is then calculated using Eq. 3.23.

Example 3.3 Using the Eurocode 2 approach, the ﬁnal long-term deﬂection (vC )max is to be calculated at the mid-point C in the end span of the one-way slab of Example 3.2 that is illustrated in Fig. 3.6. For convenience, details of the slab are included here: slab thickness, D = 180 mm; span = ef = 5.0 m; clear cover = 20 mm; dead load (including self-weight), g = 6.4 kPa; live load, q = 3.0 kPa; short-term expected live load, q1 = 2.1 kPa; sustained part of the live load, q2 = 1.2 kPa; the deﬂection requirement, (vC )max ≤ ef /500 = 20 mm; and the reinforcement details are outlined in Example 3.2. The material properties are: fc = 25 MPa; ∗ = fy = 500 MPa; Ec = 26,700 MPa; Es = 200,000 MPa; n = Es /Ec = 7.5; εsh 0.0007 and the ﬁnal creep coefﬁcient is ϕ ∗ (τ ) = 2.5. The mean uniaxial tensile strength of concrete is fctm = 0.3(fc )2/3 = 2.57 MPa.

Instantaneous deﬂection – Eurocode 2 Section at mid-span C As given in Example 3.2, the maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m. With Ast = 440 mm2 /m and d = 154 mm, the second moments of area of the uncracked transformed section and the fully-cracked transformed section are Iuncr = 498 × 106 mm4 /m and Icr = 59.6 × 106 mm4 /m, respectively. The uncracked and fully cracked curvatures are therefore κuncr = Ms∗ /Ec Iuncr = 1.16 × 10−6 mm−1 and κcr = Ms∗ /Ec Icr = 9.68 × 10−6 mm−1 , respectively.

66 Design for serviceability The cracking moment is Mcr = Zfctm = 5.59×106 ×2.57 ×10−6 = 14.34 kNm/m and, with β = 1.0 for short-term loading, the distribution coefﬁcient ζ is obtained from Eq. 3.24b: ζ = 1−β

Mcr Ms∗

2

= 1 − 1.0 × (14.34/15.4)2 = 0.133

The instantaneous curvature at mid-span is obtained from Eq. 3.23 as: (κi )C = 0.133 × 9.68 × 10−6 + (1 − 0.133) × 1.16 × 10−6 = 2.29 × 10−6 mm−1 Section at continuous support B At this critical section, Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d = 154 mm, Iuncr = 500 × 106 mm4 /m, Icr = 72.2 × 106 mm4 /m and Mcr = 14.46 kNm/m. The uncracked and fully-cracked curvatures at B are therefore κuncr = −1.68 × 10−6 mm−1 and κcr = −11.67 × 10−6 mm−1 , respectively. From Eq. 3.24b, ζ = 1 − 1.0 × (14.46/22.5)2 = 0.587 and the instantaneous curvature at B is: (κi )B = 0.587 × (−11.67 × 10−6 ) + (1 − 0.587) × (−1.68 × 10−6 ) = −7.54 × 10−6 mm−1 Deﬂection at mid-span The instantaneous deﬂection at mid-span due to the full service load is again obtained from Eq. 3.7b as: (vC )i. max = =

2 (κA + 10 κC + κB ) 96 50002 (0 + 10 × 2.29 × 10−6 − 7.54 × 10−6 ) = 4.0 mm 96

of which, the instantaneous deﬂection due to the sustained load is 3.6 mm and the remaining instantaneous deﬂection due to the transient live load is (vC )i.(q1−q2) = 0.4 mm.

Time-dependent deﬂection due to sustained loads – Eurocode 2 The effective modulus of the concrete is obtained from Eq. 3.25 as: Ee =

26700 = 7630 MPa 1 + 2.5

and the effective modular ratio ne = Es /Ee = 26.2. With the effective modular ratio, the revised section properties of the uncracked and cracked transformed cross-sections at the mid-span and at the continuous support are required.

Design for serviceability Section at mid-span C With the reinforcement area transformed into an equivalent area of the softened concrete (due to creep) using the effective modular ratio, the second moments of area of the uncracked and fully-cracked cross-sections are Iuncr = 529 × 106 mm4 /m and Icr = 166 × 106 mm4 /m, respectively. Due to the sustained loads (wsus = g + q2 = 7.6 kPa), the moment at the section at mid-span is (MC )sus = 13.77 kNm/m and the time-dependent curvatures allowing for creep are κuncr = (MC )sus /Ee Iuncr = 3.41 × 10−6 mm−1 and κcr = (MC )sus /Ee Icr = 10.8 × 10−6 mm−1 . With Mcr = 14.34 kNm/m and with β = 0.5 for long-term loading, the distribution coefﬁcient ζ is obtained from Eq. 3.24b:

2 Mcr ζ = 1−β = 1 − 0.5 × (14.34/13.77)2 = 0.458 (MC )sus The long-term load-induced curvature at mid-span (including creep) is obtained from Eq. 3.23 as: (κsus )C = 0.458 × 10.8 × 10−6 + (1 − 0.458) × 3.41 × 10−6 = 6.82 × 10−6 mm−1 Section at continuous support B At this critical section, the revised second moments of area are Iuncr = 539 × 106 mm4 /m and Icr = 197 ×106 mm4 /m. The sustained moment at B is (MB )sus = −20.12 kNm/m and the time-dependent curvatures allowing for creep are κuncr = (MB )sus /Ee Iuncr = −4.89 × 10−6 mm−1 and κcr = −13.4 × 10−6 mm−1 . From Eq. 3.24b, ζ = 1 − 0.5 × (14.46/20.12)2 = 0.742 and, the long-term load-induced curvature at B is: (κsus )B = 0.742 × (−13.4 × 10−6 ) + (1 − 0.742) × (−4.89 × 10−6 ) = −11.2 × 10−6 mm−1 Deﬂection at mid-span The time-dependent deﬂection at mid-span due to the sustained loads plus creep is obtained from Eq. 3.7b as: (vC )sus = =

2 ((κsus )A + 10 (κsus )C + (κsus )B ) 96 50002 (0 + 10 × 6.82 × 10−6 − 11.2 × 10−6 ) = 14.8 mm 96

Time-dependent deﬂection due to shrinkage – Eurocode 2 Section at mid-span C As for the creep analysis, the second moments of area of the uncracked and fullycracked cross-sections are Iuncr = 529 × 106 mm4 /m and Icr = 166 × 106 mm4 /m,

67

68 Design for serviceability respectively, and the ﬁrst moment of area of the reinforcement about the centroidal axis of the uncracked and fully-cracked cross-sections are Suncr = 26.5 × 103 mm3 /m and Scr = 46.1 × 103 mm3 /m, respectively. The shrinkageinduced curvatures are obtained from Eq. 3.26: (κsh )uncr = εsh ne

Suncr = 0.92 × 10−6 mm−1 Iuncr

and (κsh )cr = εsh ne

Scr = 5.09 × 10−6 mm−1 Icr

With ζ = 0.458, as for in the creep analysis, the shrinkage-induced curvature at mid-span is obtained from Eq. 3.23 as: (κsh )C = 0.458 × 5.09 × 10−6 + (1 − 0.458) × 0.92 × 10−6 = 2.82 × 10−6 mm−1 At the supports At the discontinuous support A, the member is uncracked and so (κsh )A = 0.92 × 10−6 mm−1 . In the negative moment region, adjacent to support B, the slab contains both top and bottom reinforcement and Suncr = −6.2 × 103 mm3 /m, Iuncr = 588×106 mm4 /m, Scr = −46.9×103 mm3 /m and Icr = 204×106 mm4 /m. Therefore, from Eq. 3.26: (κsh )uncr = −0.19×10−16 mm−1 and (κsh )cr = −4.22× 10−6 mm−1 . With ζ = 0.742, Eq. 3.23 gives (κsh )B = −3.18 × 10−6 mm−1 . Shrinkage-induced deﬂection at mid-span An estimate of the shrinkage-induced deﬂection is obtained by assuming a parabolic distribution of shrinkage curvature between the end sections and mid-span. Eq. 3.7b gives: (vC )sh = =

2 ((κsh )A + 10 (κsh )C + (κsh )B ) 96 50002 (0.92 + 10 × 2.82 − 3.18) × 10−6 = 6.8 mm 96

The ﬁnal long-term deﬂection – Eurocode 2 The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.q1−q2 + (vC )sus + (vC )sh = 0.4 + 14.8 + 6.8 = 22.0 mm = span/227

Design for serviceability

69

Discussion This result is in reasonable agreement with the ﬁnal deﬂection calculated in Example 3.2 using AS 3600-2009, although a little more conservative. Unlike AS 3600-2009 (and ACI 318-08), the approach provides a rational consideration of the long-term deﬂection due to creep and shrinkage of the concrete. Of course, the ﬁnal deﬂection here is heavily dependent on input values of the creep coefﬁcient and the shrinkage strain of concrete – as is the case in real slabs. The use of the mean concrete tensile strength fctm instead of the ﬂexural strength indirectly compensates for the tension induced by restrained shrinkage (Ref. 24). It is of interest to note that deemed-to-comply maximum span-to-depth ratios in Eurocode 2 (Eqs 3.2) suggest that, if a slab thickness greater than 173 mm was selected (see Example 3.1), then the maximum ﬁnal long-term deﬂection will not exceed span/250 and deﬂections need not be calculated. This example suggests that this is not the case and that Eqs 3.2 cannot be relied on to guarantee adequate serviceability.

3.6.6 Recommended simpliﬁed approach It is well known that Branson’s Equation (Eq. 3.18) overestimates stiffness after cracking for members containing relatively small quantities of tensile reinforcement (Refs 18, 25 and 26). A much better model for Ief can be developed from the deﬂection calculation approach in Eurocode 2 (as outlined in Section 3.6.5). Substituting Eq. 3.24b into Eq. 3.23, the instantaneous curvature at a particular section in the cracked region of a member may be calculated from:

Mcr 2 Mcr 2 κ = 1−β κcr + β κuncr (3.27) Ms∗ Ms∗ Using the notation of Eq. 3.18, the curvatures in Eq. 3.27 are κ = Ms∗ /Ec Ief , κcr = Ms∗ /Ec Icr and κuncr = Ms∗ /Ec Iuncr and Eq. 3.27 can be re-expressed as:

∗

Ms∗ Mcr 2 Ms Mcr 2 Ms∗ = 1−β + β (3.28) Ec Ief Ms∗ Ec Icr Ms∗ Ec Iuncr Eq. 3.28 can be rearranged to give the following expression for Ief : Ief =

1−β 1−

Icr Icr Iuncr

Mcr Ms∗

2 ≤ Ief .max

(3.29)

This alternative expression for Ief was ﬁrst proposed by Bischoff (Ref. 25). 3.6.6.1 Instantaneous deﬂection The instantaneous curvature κi due to the service moment Ms∗ at a particular crosssection is κi = Ms∗ /Ec Ief , with Ief calculated from Eq. 3.29, where Icr is the second moment of area of the fully-cracked section about its centroidal axis; Iuncr is the

70 Design for serviceability second moment of area of the uncracked transformed cross-section about its centroidal axis; Ms∗ is the maximum bending moment at the section, based on the short-term serviceability design load or the construction load; Mcr is the cracking moment given by + P/Ag ) + Pe ≥ 0.0 Mcr = Z(fct.f

(3.30)

where Z is the section modulus of the uncracked section, referring to the extreme (= 0.6 f ) is the characteristic ﬂexural tensile ﬁbre at which cracking occurs; and fct.f c strength of concrete. An upper limit Ief .max is recommended for the value of Ief calculated from Eq. 3.29, where Ief .max = Iuncr when p = Ast /bd ≥ 0.005 and Ief .max = 0.6Iuncr when p < 0.005. For lightly reinforced members (where ρ < 0.005), the value of Ief is very sensitive to the calculated value of Mcr . The ratio Iuncr /Icr is large and the maximum in-service moment Ms∗ may be similar in magnitude to the cracking moment. An upper limit for Ief of 0.6Iuncr is imposed on such members, because failure to account for cracking due to unanticipated shrinkage restraint, temperature gradients or construction loads can result in signiﬁcant underestimates of deﬂection. The term β in Eq. 3.29 is used to account for both shrinkage-induced cracking and the reduction in tension stiffening with time. Early shrinkage in the days and weeks after casting will cause tension in the concrete and a reduction in the cracking moment. As time progresses and the concrete continues to shrink, the level of shrinkage-induced tension increases in an uncracked member, further reducing the cracking moment. If shrinkage has not occurred before ﬁrst loading, the deﬂection immediately after loading may be calculated with β = 1.0. However, in practice, signiﬁcant shrinkage usually occurs before ﬁrst loading and β is less than 1.0. When calculating the shortterm or elastic part of the deﬂection, the following is recommended: β = 0.7 β = 0.5

at early ages (less than 28 days); and at ages greater than 6 months.

For long-term calculations, when the ﬁnal deﬂection is to be estimated, β = 0.5 should be used. The instantaneous deﬂection is calculated by assuming a uniform average rigidity for the span of Ec (Ief )av . For a simple-supported beam or slab, the average value (Ief )av for the span is determined from the value of Ief at mid-span. For interior spans of continuous beams or slabs, (Ief )av is taken to be half the mid-span value plus one quarter of the value at each support. For end spans of continuous beams or slabs, (Ief )av is taken to be half the mid-span value plus half the value at the continuous support. For a cantilever, (Ief )av is the value at the support. 3.6.6.2 Time-dependent creep-induced curvature The creep-induced curvature κcr (t) on a particular cross-section at any time t due to a sustained service load ﬁrst applied at age τ0 may be obtained from: κcr (t) = κsus,0

ϕ(t, τ0 ) α

(3.31)

Design for serviceability

71

where κsus,0 is the instantaneous curvature due to the sustained service loads; ϕ(t, τ0 ) is the creep coefﬁcient at time t due to load ﬁrst applied at age τ0 ; and α is a creep modiﬁcation factor that accounts for the effects of cracking and the braking action of the reinforcement on creep and may be estimated from either Eqs 3.32a, b or c (Refs 26 and 30). For a cracked reinforced concrete section in pure bending (Ief < Iuncr ), α = α1 , where:

α1 = 0.48ρ

−0.5

I 0.33 Asc 1.2 cr 1 + (125ρ + 0.1) Ief Ast

(3.32a)

For an uncracked reinforced or prestressed concrete section (Ief = Iuncr ), α = α2 , where: Asc (3.32b) α2 = 1.0 + 45ρ − 900ρ 2 1 + Ast and ρ = Ast /bdo ; Ast is the equivalent area of bonded reinforcement in the tensile zone at depth do (the depth from the extreme compressive ﬁbre to the centroid of the outermost layer of tensile reinforcement); and Asc is the area of the bonded reinforcement in the compressive zone between the neutral axis and the extreme compressive ﬁbre. The area of any bonded reinforcement in the tensile zone (including bonded tendons) not contained in the outermost layer of tensile reinforcement (i.e. located at a depth d1 less than do ) should be included in the calculation of Ast by multiplying that area by d1 /do . For the purpose of the calculation of Ast , the tensile zone is that zone that would be in tension due to the applied moment acting in isolation. For a cracked, partially prestressed section or for a cracked reinforced concrete section subjected to bending and axial compression, α may be taken as:

dn1 α = α2 + (α1 − α2 ) dn

2.4 (3.32c)

where dn is the depth of the intact compressive concrete on the cracked section and dn1 is the depth of the intact compressive concrete on the cracked section ignoring the axial compression and/or the prestressing force (i.e. the value of dn for an equivalent cracked reinforced concrete section in pure bending containing the same quantity of bonded reinforcement). 3.6.6.3 Time-dependent shrinkage-induced curvature The shrinkage-induced curvature on a reinforced concrete section is approximated by:

κsh =

kr εsh D

(3.33)

where D is the overall depth of the section; εsh is the shrinkage strain; and kr depends on the quantity and location of bonded reinforcement Ast and Asc , and may be estimated from Eqs 3.34a–d, as appropriate (Ref. 30).

72 Design for serviceability For a cracked reinforced concrete section in pure bending (Ief < Iuncr ), kr = kr1 , where:

Icr kr1 = 1.2 Ief

0.67 1 − 0.5

Asc Ast

D do

(3.34a)

For an uncracked cross-section (Ief = Iuncr ), kr = kr2 , where:

do Asc 1.3 −1 1− when ρ = Ast /bdo ≤ 0.01 0.5D Ast (3.34b)

1.3

do Asc kr2 = (40ρ + 0.35) when ρ = Ast /bdo > 0.01 (3.34c) −1 1− 0.5D Ast

kr2 = (100ρ − 2500ρ 2 )

In Eqs 3.34a, b and c, Asc is deﬁned as the area of the bonded reinforcement on the compressive side of the cross-section. This is a different deﬁnition to that provided under Eq. 3.32b. While bonded steel near the compressive face of a cracked crosssection that is at or below the neutral axis will not restrain compressive creep, it will provide restraint to shrinkage and will affect the shrinkage-induced curvature on a cracked section. For a cracked, partially prestressed section or for a cracked reinforced concrete section subjected to bending and axial compression, kr may be taken as: kr = kr2 + (kr1 − kr2 )

dn1 dn

(3.34d)

where dn and dn1 are as deﬁned after Eq. 3.32c. Eqs 3.32, 3.33 and 3.34 have been developed (see Ref. 30) as empirical ﬁts to results obtained from a parametric study of the creep- and shrinkage-induced changes in curvature on reinforced concrete cross-sections under constant sustained internal actions using the age-adjusted effective modulus method (AEMM) of analysis (as outlined subsequently in Chapter 5).

Example 3.4 Using the approach recommended above (Eqs 3.29–3.34), the ﬁnal long-term deﬂection (vC )max is to be calculated at the mid-point C in the end span of the one-way slab of Example 3.2 that was illustrated in Fig. 3.6. For convenience, details of the slab are included here: h = 180 mm; = ef = 5.0 m; clear cover = 20 mm; dead load (including self-weight), g = 6.4 kPa; live load, q = 3.0 kPa; short-term expected live load, q1 = 2.1 kPa; sustained live load, q2 = 1.2 kPa; and (vC )max ≤ ef /500 = 20 mm. The reinforcement details are outlined in Example 3.2 and shown in Fig. 3.6a; and the bending moment diagram under the maximum uniformly distributed service load, wmax = g + q1 = 8.5 kPa is shown in Fig. 3.6b.

Design for serviceability The material properties are fc = 25 MPa; fct.f 3.0 MPa; fy = 500 MPa; ∗ = 0.0007 and Ec = 26,700 MPa; Es = 200,000 MPa; n = Es /Ec = 7.5; εsh ∗ ϕ (τ ) = 2.5.

Instantaneous deﬂection Section at mid-span C The maximum in-service moment at mid-span is Ms∗ = 15.4 kNm/m and with Ast = 440 mm2 /m, d = 154 mm and p = 0.00286, the second moments of area of the uncracked transformed section and the fully-cracked transformed section are Iuncr = 498 × 106 mm4 /m and Icr = 59.6 × 106 mm4 /m, respectively. The = 5.59 × 106 × 3.0 × 10−6 = 16.8 kNm/m and, cracking moment is Mcr = Zfct.f for the calculation of immediate deﬂection due to loads applied at any time after shrinkage-induced cracking has occurred, take β = 0.5. The value of Ief for the section at mid-span is obtained from Eq. 3.29:

Ief =

59.6 × 106

1 − 0.5 1 −

59.6 × 106

498 × 106

16.8 15.4

6 4

2 = 125 × 10 mm /m

Section at continuous support B At this critical section, Ms∗ = −22.5 kNm/m, Ast = 550 mm2 /m, d = 154 mm, Iuncr = 500 × 106 mm4 /m, Icr = 72.2 × 106 mm4 /m, Mcr = 16.9 kNm/m and therefore: Ief =

72.2 × 106

72.2 × 106 1 − 0.5 1 − 500 × 106

16.9 22.5

6 4

2 = 95.3 × 10 mm /m

Short-term deﬂection at mid-span The average value (Ief )av for the span is taken as one half the value of Ief at mid-span plus half the value at the continuous support. That is (Ief )av = 0.5 (125 + 95.3) × 106 = 110 × 106 mm4 /m. The instantaneous curvature at midspan and at support B are (κi )C = Ms∗ /Ec (Ief )av = (15.4 × 106 )/(26,700 × 110 × 106 ) = 5.24 × 10−6 mm−1 and (κi )B = Ms∗ /Ec (Ief )av = (−22.5 × 106 )/(26,700 × 110 × 106 ) = −7.66 × 10−6 mm−1 , respectively. The instantaneous deﬂection at mid-span due to the full service load is obtained from Eq. 3.7b as: (vC )i. max = =

2 ((κi )A + 10 (κi )C + (κi )B ) 96 50002 (0 + 10 × 5.24 × 10−6 − 7.66 × 10−6 ) = 11.7 mm 96

73

74 Design for serviceability

Time-dependent deﬂection Creep The sustained service load is wsus = g + q2 = 7.6 kPa = 0.894wmax , and therefore the sustained moments at mid-span and at the continuous support are Msus = 13.8 kNm/m and −20.1 kNm/m, respectively. The instantaneous curvatures at mid-span and at the continuous support due to the sustained loads (κsus,0 = Msus /Ec Ief .av ) are therefore 4.68 × 10−6 mm−1 and −6.85 × 10−6 mm−1 , respectively. The creep modiﬁcation factor α for the sections at mid-span and at the continuous support are obtained from Eq. 3.32a as α = α1 = [0.48 × 0.00286−0.5 ] × [59.6 × 106 /125 × 106 ]0.33 = 7.0 and α = α1 = [0.48 × 0.00357−0.5 ] × [72.2 × 106 /95.3 × 106 ]0.33 = 7.3, respectively. For the cross-section at the continuous support, the bottom (compressive) steel is not located in the compressive zone of the cracked section and so Asc in Eq. 3.32a is zero. From Eq. 3.31 the ﬁnal creep-induced curvature at the mid-span C and at the continuous support B are (κcr )C = 4.68×10−6 ×2.5/7.0 = 1.67×10−6 mm−1 and (κcr )B = −6.85 × 10−6 × 2.5/7.3 = −2.35 × 10−6 mm−1 , respectively. From Eq. 3.7b, the creep-induced deﬂection is: (vC )cr = =

2 ((κcr )A + 10 (κcr )C + (κcr )B ) 96 50002 (0 + 10 × 1.67 × 10−6 − 2.35 × 10−6 ) = 3.7 mm 96

Shrinkage For the cracked cross-section at mid-span, Eq. 3.34a gives kr = kr1 = 1.2 × (59.6 × 106 /125 × 106 )0.67 × 180/154 = 0.85 and the shrinkage-induced curvature is given by Eq. 3.33, (κsh )C = 0.85×0.0007/180 = 3.32×10−6 mm−1 . For the cracked section at the continuous support, Asc = 440 mm2 /m in Eq. 3.34a and kr = kr1 = 1.2 × (72.2 × 106 /95.3 × 106 )0.67 × (1 − 0.5 × 440/550) × (180/154) = 0.70 and the shrinkage-induced curvature is given by Eq. 3.33: (κsh )B = −0.70 × 0.0007/180 = −2.72 × 10−6 mm−1 . For the uncracked, singlyreinforced section at support A, Eq. 3.34b gives kr = kr2 = (100 × 0.00286 − 2500 × 0.002862 ) × (154/90 − 1) = 0.19 and, from Eq. 3.33, (κsh )A = 0.19 × 0.0007/180 = 0.74 × 10−6 mm−1 . If shrinkage-induced deﬂection is obtained by assuming a parabolic distribution of shrinkage curvature between the end sections and mid-span, Eq. 3.7b gives: (vC )sh = =

2 ((κsh )A + 10 (κsh )C + (κsh )B ) 96 50002 (0.74 + 10 × 3.32 − 2.72) × 10−6 = 8.1 mm 96

Design for serviceability

75

The ﬁnal long-term deﬂection The ﬁnal long-term deﬂection at mid-span (vC )max is therefore: (vC )max = (vC )i.max + (vC )cr + (vC )sh = 11.7 + 3.7 + 8.1 = 23.5 mm = span/213 Discussion The ﬁnal deﬂection calculated here is similar to that calculated in Example 3.3 using the procedure in Eurocode 2. However, this is not necessarily the case in all situations. The procedure described in Section 3.6.6 is considered to be the most reliable of the simpliﬁed procedures presented in this chapter and will generally provide a conservative estimate of deﬂections.

3.7 Crack control 3.7.1 General Reinforced concrete elements crack wherever the tensile stress in the concrete reaches the tensile strength of the concrete. Tensile stress at any location in a concrete structure may be caused by a number of factors, including applied loads, restrained shrinkage, temperature changes, settlement of supports and so on. Cracks formed by axial tensile forces and restrained shrinkage (direct tension cracks) often penetrate completely through a member. Cracks caused by bending (ﬂexural cracks) occur at the tensile face when the extreme ﬁbre tensile stress reaches the tensile strength of the concrete. Flexural cracks propagate from the extreme tensile ﬁbre through the tensile zone and are arrested at or near the neutral axis. Flexural cracks increase in width as the distance from the tensile reinforcement increases and taper to zero width near the neutral axis. A linear relationship is generally assumed to exist between the crack width at the side or sofﬁt of a member and the distance from the bar. In general, the spacing between ﬂexural cracks is in the range 0.5 to 1.5 times the depth of the member. Many variables inﬂuence the width and spacing of cracks, including the magnitude and duration of loading, the quantity, orientation and distribution of the reinforcement, the cover to the reinforcement, the slip between the reinforcement and the concrete in the vicinity of the crack (that depends on the bond characteristics of the reinforcement), the deformational properties of the concrete (including its creep and shrinkage characteristics) and the size of the member. Considerable variations exist in the crack width from crack to crack and the spacing between adjacent cracks because of random variations in the properties of concrete. The control of cracking in concrete structures is usually achieved by limiting the stress in the bonded reinforcement crossing a crack to some appropriately low value and ensuring that the bonded reinforcement is suitably distributed within the tensile zone. The limit on the tensile steel stress imposed in design depends on the maximum acceptable crack width. Typical values for maximum acceptable crack widths were given in Table 3.2 in Section 3.4.2. If the maximum acceptable crack

76 Design for serviceability width is increased, the maximum permissible tensile steel stress also increases. Building codes usually specify maximum bar spacings for the bonded reinforcement and maximum concrete cover requirements. Some codes specify deterministic procedures for calculating crack widths, with the intention to control cracking by limiting the calculated crack width to some appropriately low value. However, current design procedures to control cracking using conventional steel reinforcement are often overly simplistic and fail to adequately account for the gradual increase in crack widths with time due to shrinkage. In Chapter 1, Section 1.3.3, the restraint provided to shrinkage by the bonded reinforcement in a reinforced concrete member was discussed, with the concrete compressing the reinforcement as it shrinks and the reinforcement imposing an equal and opposite tensile force on the concrete at the level of the steel (as shown in Fig. 1.14b). This internal tensile restraining force is often signiﬁcant enough to cause time-dependent cracking. In addition, the connections of a concrete member to other parts of the structure or to the foundations also provide restraint to shrinkage. The tensile restraining force that develops rapidly with time at the restrained ends of the member usually leads to cracking, often within days of the commencement of drying. In a restrained ﬂexural member, shrinkage also causes a gradual widening of ﬂexural cracks and a gradual build-up of tension in the uncracked regions that may lead to additional cracking. The inﬂuence of shrinkage on crack widths is not properly considered in the major building codes and is therefore not adequately considered in structural design. As a consequence, excessively wide cracks are a relatively common problem for many reinforced concrete structures. 3.7.2 Simpliﬁed code-oriented approaches for ﬂexural crack control Many simpliﬁed approaches for crack control in reinforced concrete are available in the literature. Some of the more commonly used methods are presented and evaluated here. 3.7.2.1 Gergely and Lutz (Ref. 31) Based on a statistical analysis of experimental data, Gergely and Lutz proposed the following expression for the maximum crack width w (mm) at the tensile face of a beam or slab containing deformed bars: w = 0.011

D − kd σst1 (c1 A)0.33 × 10−3 d − kd

(3.35)

where c1 is the concrete cover measured from the tensile face to the centre of the longitudinal bar closest to that face (mm); A is the concrete area surrounding each longitudinal bar and may be taken as the total effective area of the concrete in the tensile zone of the cross-section having the same centroid as the tensile reinforcement divided by the number of longitudinal bars (mm2 ); σst1 is the tensile steel stress at the crack (MPa); D is the overall depth of the cross-section; d is the effective depth deﬁned as the distance from the compressive edge of the cross-section to the centroid of the tensile reinforcement; and kd is the depth from the compressive edge to the neutral axis of the cracked section.

Design for serviceability

77

3.7.2.2 Frosch (Ref. 32) The following alternative expression for the maximum crack width w (mm) at the tensile face of a beam or slab containing deformed bars was proposed by Frosch: w=2

σst1 D − kd 2 c1 + (sb /2)2 Es d − kd

(3.36)

where sb is the maximum bar spacing (mm); and Es is the elastic modulus of the steel (MPa). 3.7.2.3 Eurocode 2 – 1992 (Ref. 5) According to the 1992 version of Eurocode 2, the design crack width may be calculated from:

σst1 σsr 2 1 − β1 β2 (3.37) w = β srm Es σst1 where β1 = 1.0 for deformed bars and 0.5 for plain bars; β2 = 1.0 for a single, shortterm load and 0.5 for repeated or sustained loading; σsr is the stress in the tensile reinforcement at the loading causing ﬁrst cracking calculated ignoring the concrete in tension; σst1 is the stress in the reinforcement at the loading under consideration calculated ignoring the concrete in tension; β is the ratio of the design crack width to the average crack width taken as β = 1.7 for load-induced cracking and, for cracking due to restrained shrinkage, β = 1.3 when the minimum dimension of the member is less than 300 mm and increases to β = 1.7 when the minimum dimension is 800 mm or greater; srm is the average crack spacing given by: srm = 50 + 0.25 k1 k2 db /ρeff

(3.38)

in which k1 is a coefﬁcient equal to 0.8 for deformed bars and 1.6 for plain round bars; k2 is a coefﬁcient that takes into account the form of the strain distribution on the cross-section and equals 0.5 for bending and 1.0 for direct tension; db is the average bar diameter for the tensile reinforcement; and ρeff is the effective reinforcement ratio, Ast /Ac.eff ; Ast is the area of tensile reinforcement; and Ac.eff is the effective area of the tensile concrete surrounding the tensile reinforcement of depth equal to 2.5 times the distance from the tension face of the section to the centroid of the tensile reinforcement (i.e. 2.5(D − d)), but not greater than (D − kd)/3 or D/2. 3.7.2.4 Eurocode 2 – 2004 (Ref. 6) In the 2004 version of Eurocode 2, the crack width in a reinforced concrete member is calculated from: w = sr,max (εsm − εcm )

(3.39)

where sr,max is the maximum crack spacing; εsm is the mean strain in the reinforcement at the design loads, including the effects of tension stiffening and any imposed

78 Design for serviceability deformations; εcm is the mean strain in the concrete between the cracks. The difference between the mean strain in the reinforcement and the mean strain in the concrete may be taken as: εsm − εcm =

fct,eff σst1 σst1 − kt (1 + n ρeff ) ≥ 0.6 Es Es ρeff Es

(3.40)

where kt is a factor that depends on the duration of load and equals 0.6 for shortterm loading and 0.4 for long-term loading; n is the modular ratio Es /Ec ; fct,eff is the mean value of the axial tensile strength of concrete at the time cracking is expected; ρeff (= As /Ac,eff ) and Ac,eff are deﬁned under Eq. 3.38. For reinforced concrete sections with bonded reinforcement ﬁxed at reasonably close centres, the maximum ﬁnal crack width may be calculated from: sr,max = 3.4c + 0.425 k1 k2 db /ρeff

(3.41)

in which c is the clear cover to the longitudinal reinforcement; and k1 and k2 are deﬁned under Eq. 3.38. Alternatively, cracking is deemed to be controlled by Eurocode 2 (2004) if the quantity of tensile reinforcement in a beam or slab is greater than the minimum value given in Eq. 3.42 and if either the bar diameter and/or the bar spacing is limited to the maximum values given in Tables 3.7 and 3.8, respectively. The minimum area of steel for crack control is As,min = kc fct,eff Act /fs

(3.42)

where kc depends on the stress distribution prior to cracking and equals 1.0 for pure tension and 0.4 for pure bending; Act is the cross-sectional area of concrete in the tensile zone, i.e. the area in tension just before the formation of the ﬁrst crack; and fs is the maximum stress permitted in the reinforcement immediately after crack formation and is the lesser of the yield stress fy and the value given in Table 3.7. If the area of steel in the tension zone exceeds the minimum value given by Eq. 3.42, cracking is deemed to be controlled if either Tables 3.7 or 3.8 are satisﬁed. The steel stress used in these tables is the steel stress on the cracked section due to the quasipermanent loads. Table 3.7 Maximum bar diameters db for crack control (Ref. 6) Steel stress (MPa)

160 200 240 280 320 360 400 450

Maximum bar diameter (mm) Crack width, w = 0.4 mm

Crack width, w = 0.3 mm

Crack width, w = 0.2 mm

40 32 20 16 12 10 8 6

32 25 16 12 10 8 6 5

25 16 12 8 6 5 4 –

Design for serviceability

79

Table 3.8 Maximum bar spacing for crack control (Ref. 6) Steel stress (MPa)

Maximum bar spacing (mm) Crack width, w = 0.4 mm

Crack width, w = 0.3 mm

Crack width, w = 0.2 mm

300 300 250 200 150 100

300 250 200 150 100 50

200 150 100 50 – –

160 200 240 280 320 360

3.7.2.5 ACI 318-08 (Ref. 4) For the control of ﬂexural cracking in beams and one-way slabs in normal exposure conditions, ACI 318-08 requires the following. (i) The area of tensile steel provided at every cross-section should be greater than Ast.min where: 0.25 fc Ast. min = bw d ≥ 1.4bw d/fy fy

(3.43)

(ii) The ﬂexural tensile reinforcement is well distributed within the tensile zone of the cross-section and the spacing of the reinforcing bars closest to the tensile face is less than that given by: s = 380

280 280 − 2.5c ≤ 300 σst1 σst1

(3.44)

where c is the smallest distance from the surface of the reinforcement to the tensile face (mm); σst1 is the calculated stress at the crack in the reinforcement closest to the tensile face at the maximum service load (MPa), but it is permissible to take σst1 = 0.67fy . For two-way slabs, ACI 318-08 requires that the spacing of the reinforcement in each direction in a solid slab not exceed two times the slab thickness.

Example 3.5 The maximum crack width determined using Eqs 3.35, 3.36, 3.37 and 3.39 are here compared with the measured maximum ﬁnal crack widths for 12 prismatic, one-way, singly reinforced concrete specimens (six beams and six slabs) that were tested by Gilbert and Nejadi (Ref. 35) under sustained service loads for periods in excess of 400 days. The specimens were simply-supported over a span of 3.5 m with cross-sections shown in Fig. 3.7. All specimens were cast from the same

80 Design for serviceability batch of concrete and moist cured prior to ﬁrst loading at age 14 days. Details of each test specimen are given in Table 3.9. The time-dependent development of cracking, including the crack spacing and crack width, was measured in each specimen throughout the test. The measured elastic modulus and compressive strength of the concrete at the age of ﬁrst loading were Ec = 22,820 MPa and fc = 18.3 MPa, whilst the measured creep coefﬁcient and shrinkage strain associated with the 400-day period of sustained loading were ϕ(t, τ ) = 1.71 and εsh = −0.000825. Two identical specimens ‘a’ and ‘b’ were constructed for each combination of parameters as indicated in Table 3.9, with the ‘a’ specimens loaded more heavily than the ‘b’ specimens. The ‘a’ specimens were subjected to a constant sustained load sufﬁcient to cause a maximum moment at mid-span of between 40 and 50 per cent of the calculated ultimate moment and the ‘b’ specimens were subjected to a constant sustained mid-span moment of between 25 and 40 per cent of the calculated ultimate moment.

250 mm

400 mm 300 mm sb

sb

cb

cb

130 mm

Ast

Ast cs

cs (a) Beams

(b) Slabs

Figure 3.7 Cross-sections of test specimens (Ref. 35).

Table 3.9 Details of the test specimens (Ref. 35) Beam No. of db Ast cs sb cb bars (mm) (mm2 ) (mm) (mm) (mm)

Slab No. of db Ast cs sb cb bars (mm) (mm2 ) (mm) (mm) (mm)

B1-a B1-b B2-a B2-b B3-a B3-b

S1-a S1-b S2-a S2-b S3-a S3-b

2 2 2 2 3 3

16 16 16 16 16 16

400 400 400 400 600 600

40 40 25 25 25 25

40 40 25 25 25 25

154 154 184 184 92 92

2 2 3 3 4 4

12 12 12 12 12 12

226 226 339 339 452 452

25 25 25 25 25 25

40 40 40 40 40 40

308 308 154 154 103 103

The loads on all specimens were sufﬁcient to cause primary cracks to develop in the region of maximum moment at ﬁrst loading. In Table 3.10, the sustained in-service moment at mid-span, Msus , is presented, together with the stress in the tensile steel at mid-span, σst1 , due to Msus (calculated on the basis of a

Design for serviceability

81

fully cracked section); the calculated ultimate ﬂexural strength, Mu (assuming a characteristic yield stress of the reinforcing steel of 500 MPa); the ratio Msus /Mu ; and the cracking moment, Mcr (calculated assuming a tensile strength of concrete of 0.6 fc (t), where fc (t) is the measured compressive strength at the time of loading in MPa).

Table 3.10 Moments and steel stresses in the test specimens (Ref. 35) Beam Mcr Msus σst1 Mu Msus /Mu (kNm) (kNm) (MPa) (kNm) (%)

Slab Mcr Msus σst1 Mu Msus /Mu (kNm) (kNm) (MPa) (kNm) (%)

B1-a B1-b B2-a B2-b B3-a B3-b

S1-a S1-b S2-a S2-b S3-a S3-b

14.0 14.0 13.1 13.1 13.7 13.7

24.9 17.0 24.8 16.8 34.6 20.8

227 155 226 153 214 129

56.2 56.2 56.2 56.2 81.5 81.5

44.3 30.2 44.1 29.8 42.4 25.5

4.65 4.65 4.75 4.75 4.86 4.86

6.81 5.28 9.87 6.81 11.4 8.34

252 195 247 171 216 159

13.9 13.9 20.3 20.3 26.4 26.4

49.0 38.0 48.6 33.6 43.0 31.6

At ﬁrst loading, a regular pattern of primary cracks developed in each test specimen. With time, the cracks gradually increased in width and additional cracks developed between some of the primary cracks. Thus, the average crack spacing reduced with time. The ratio of ﬁnal to initial crack spacing ranged from 0.57 to 0.85, with an average value of 0.70. Crack widths increased rapidly in the ﬁrst few weeks after loading, but the rate of increase slowed signiﬁcantly after about 2 months. For all specimens, there was little change in the maximum crack width after about 200 days under load. Typical calculations for the maximum crack width are provided here for Beam B2-a. Beam B2-a: Typical maximum crack width calculations are provided here for Beam B2-a, with b = 250 mm, D = 333 mm, d = 300 mm, Ast = 400 mm2 , Ec = 22820 MPa, n = Es /Ec = 8.76. A cracked section analysis gives kd = 78.8 mm and Icr = 212 × 106 mm4 . The applied moment at mid-span is Msus = 24.8 kN and the stress in the tensile steel on the cracked section is: σst1 =

nMsus (d − kd) 8.76 × 24.8 × 106 × (300 − 78.8) = = 226 MPa Icr 212 × 106

Gergely and Lutz: For B2-a, c1 = 33 mm, A = (250 × 66)/2 = 8250 mm2 and from Eq. 3.35: w = 0.011 ×

333 − 78.8 × 226 × (33 × 8250)0.33 = 0.178 mm 300 − 78.8

82 Design for serviceability Frosch: For B2-a, the bar spacing is sb = 184 mm and from Eq. 3.36: 226 333 − 78.8 w = 2× × × 332 + (184/2)2 = 0.254 mm 200,000 300 − 78.8 Eurocode 2 (1992): For B2-a, the additional parameters required for the Eurocode 2 (1992) approach are: β = 1.7; β1 = 1.0; β2 = 0.5 for sustained loading; fctm = 2.08 MPa; σsr = (Mcr /Ms ) σst1 = 96.8 MPa; k1 = 0.8; k2 = 0.5; Ac.eff = 2.5 × 33 × 250 = 20,625 mm2 ; ρeff = 400/20,625 = 0.0194; and srm = 50 + 0.25 × 0.8 × 0.5 × 16/0.0194 = 132 mm. From Eq. 3.37:

226 96.8 2 w = 1.7 × 132 × = 0.232 mm 1 − 1.0 × 0.5 × 200,000 226 Eurocode 2 (2004): For B2-a, the additional parameters required for the Eurocode 2 (2004) approach are: c = 25 mm; fct,eff = 2.08 MPa; and from Eq. 3.41, sr,max = 3.4×25+0.425× 0.8 × 0.5 × 16/0.0194 = 225 mm. Now σst1 /Es = 0.00113 and from Eq. 3.40: εsm − εcm = 0.00113 − 0.4 × 2.08 × (1 + 8.76 × 0.0194)/(200,000 × 0.0194) = 0.000881. From Eq. 3.39: w = 225 × 0.000881 = 0.198 mm Calculated versus measured maximum crack width: For this specimen, all four calculation methods signiﬁcantly underestimate the measured maximum ﬁnal crack width of 0.36 mm. The measured and calculated maximum ﬁnal crack widths for all 12 beam and slab specimens are compared in Table 3.11. The mean of the ratios of predicted to measured crack widths and the coefﬁcient of variation for each calculation method are also provided for both the beam and the slab specimens. For the beam specimens, all four calculation methods signiﬁcantly underestimate the measured maximum crack width. The Eurocode 2 (1992) approach has the lowest coefﬁcient of variation. None of the calculation methods adequately accounts for the very signiﬁcant time-dependent increase in crack width due to drying shrinkage. In fact, the crack width predicted by each of the methods is independent of the level of drying shrinkage or the creep coefﬁcient. For the slab specimens, the Gergely and Lutz method (Eq. 3.35) provides a reasonable estimate of maximum crack width for this set of test data. Both Eurocode 2 approaches again have the lowest coefﬁcients of variation, but underestimate the measured test data. The expression proposed by Frosch (Eq. 3.36) tends to overestimate the measured maximum crack width, particularly when the bar spacing is wide (such as in specimens S1-a and S1-b).

Design for serviceability

83

Table 3.11 Comparison of measured and predicted maximum ﬁnal crack widths (mm) Specimen Measured Gergely and Lutz (mm) (Eq. 3.35)

Frosch (Eq. 3.36)

Eurocode 2 1992 (Eq. 3.37)

Eurocode 2 2004 (Eq. 3.39)

Predicted Predicted/ Predicted Predicted/ Predicted Predicted/ Predicted Predicted/ (mm) Measured (mm) Measured (mm) Measured (mm) Measured B1-a B1-b B2-a B2-b B3-a B3-b

0.38 0.18 0.36 0.18 0.28 0.13

0.242 0.165 0.178 0.121 0.149 0.089

Mean Coefﬁcient of variation (%) S1-a S1-b S2-a S2-b S3-a S3-b

0.25 0.20 0.23 0.18 0.20 0.15

0.254 0.197 0.221 0.153 0.179 0.131

Mean Coefﬁcient of variation (%)

0.638 0.919 0.494 0.670 0.531 0.688

0.251 0.171 0.254 0.172 0.141 0.085

0.661 0.952 0.707 0.957 0.503 0.651

0.242 0.143 0.232 0.138 0.179 0.097

0.637 0.796 0.644 0.769 0.638 0.747

0.250 0.146 0.198 0.116 0.157 0.082

0.658 0.811 0.551 0.645 0.562 0.634

0.657

0.739

0.705

0.644

22.8

24.5

10.4

14.5

1.015 0.984 0.962 0.848 0.895 0.873

0.520 0.403 0.274 0.189 0.176 0.129

2.081 2.016 1.192 1.051 0.881 0.859

0.257 0.176 0.211 0.132 0.160 0.111

1.029 0.878 0.917 0.735 0.801 0.738

0.218 0.150 0.184 0.113 0.142 0.096

0.872 0.749 0.800 0.629 0.708 0.639

0.930

1.346

0.849

0.733

7.2

41.4

13.5

12.8

3.7.3 Tension chord model for ﬂexural cracking in reinforced concrete A model for predicting the maximum ﬁnal crack width (w∗ ) in reinforced concrete ﬂexural members based on the tension chord model of Marti et al. (Ref. 32) was recently proposed (Ref. 34). A modiﬁed version of that model is presented here and has been shown to provide good agreement with the measured ﬁnal spacing and width of cracks in reinforced concrete beams and slabs under sustained loads. The notation associated with the model is shown in Fig. 3.8. Consider a segment of a singly reinforced beam of rectangular section subjected to an in-service bending moment, Ms , greater than the cracking moment, Mcr . The spacing between the primary cracks is s, as shown in Fig. 3.8a. A typical cross-section between the cracks is shown in Fig. 3.8b and a cross-section at a primary crack is shown in Fig. 3.8c. The cracked beam is idealised as a compression chord of depth kd and width b and a cracked tension chord consisting of the tensile reinforcement of area Ast surrounded by an area of tensile concrete (Act ) as shown in Fig. 3.8d. The centroids of Ast and Act are assumed to coincide at a depth d below the top ﬁbre of the section. For the sections containing a primary crack (Fig. 3.8c), Act = 0 and the depth of the compressive zone, kd, and the second moment of area about the centroidal axis (Icr ) may be determined from a cracked section analysis using modular ratio theory (Eqs 3.14 and 3.17). Away from the crack, the area of the concrete in the tension chord of Fig. 3.8d (Act ) is assumed to carry a uniform tensile stress (σct ) that develops due to the bond stress (τb ) that exists between the tensile steel and the surrounding concrete.

84 Design for serviceability b

b kd d

Ms h

(1−k)d Ast

Ast s

Primary crack

(a) Beam elevation

(c) Cracked section

(b) Uncracked section

b C

C

kd d

Cracked tension chord Ts + Tc

T s

Ast Act

(d) Idealised compression and tension chord model

Figure 3.8 Cracked reinforced concrete beam and idealised tension chord model (Ref. 34).

For the tension chord, the area of concrete between the cracks, Act , may be taken as: Act = 0.5(D − kd)b∗

(3.45)

where b∗ is the width of the section at the level of the centroid of the tensile steel (i.e. at the depth d) but not greater than the number of bars in the tension zone multiplied by 12db . At each crack, the concrete carries no tension and the tensile steel stress is σst1 = T/Ast , where: T=

nMs (d − kd) Ast Icr

(3.46)

As the distance z from the crack in the direction of the tension chord increases, the stress in the steel reduces due to the bond shear stress τb between the steel and the surrounding tensile concrete. For reinforced concrete under service loads, where σst1 is less than the yield stress fy , Marti et al. (Ref. 33) assumed a rigid-plastic bond shear stress-slip relationship, with τb = 2.0fct at all values of slip, where fct is the direct tensile strength of the concrete. To account for the reduction in bond stress with time due to tensile creep and shrinkage, Gilbert (Ref. 34) took the bond stress to be τb = 2.0fct for short-term calculations and τb = 1.0fct when the ﬁnal long-term crack width was to be determined. Experimental observations (Refs 35 and 36) indicate that τb reduces as the stress in the reinforcement increases and, consequently, the tensile stresses in the concrete between the cracks reduces (i.e. tension stiffening reduces with increasing steel stress). In reality, the magnitude of τb is affected by many factors, including steel

Design for serviceability

85

stress, concrete cover, bar spacing, transverse reinforcement (stirrups), lateral pressure, compaction of the concrete, size of bar deformations, tensile creep and shrinkage. It is recommended here that in situations where the concrete cover and the clear spacing between the bars are greater than the bar diameter, the bond stress τb may be taken as: τb = λ1 λ2 λ3 fct

(3.47)

where λ1 accounts for the load duration with λ1 = 1.0 for short-term calculations and λ1 = 0.7 for long-term calculations; λ2 is a factor that accounts for the reduction in bond stress as the steel stress σst1 (in MPa) increases and is given by (Ref. 36): ˙ st1 ≥ 0.0 λ2 = 1.66˙ − 0.003σ

(3.48)

and λ3 is a factor that accounts for the very signiﬁcant increase in bond stress that has been observed in laboratory tests for small diameter bars (Ref. 35) and may be taken as: λ3 = 7.0 − 0.3db ≥ 2.0 (db in mm)

(3.49)

An elevation of the tension chord is shown in Fig. 3.9a and the stress variations in the concrete and steel in the tension chord are illustrated in Figs 3.9b and 3.9c, respectively. Following the approach of Marti et al. (Ref. 33), the concrete and steel tensile stresses in Figs 3.9b and 3.9c, where 0 < z ≤ s/2, may be expressed as: σstz =

T 4τ z − b Ast db

(3.50a)

tb T Crack

s/2

Crack

s/2

(a) Elevation of tension chord between cracks z

sc2

(b) Tensile concrete stress sst1

sst1 sst2

(c) Tensile steel stress

Figure 3.9 Tension chord – actions and stresses (Ref. 33).

86 Design for serviceability and σcz =

4τb ρtc z db

(3.50b)

where ρtc is the reinforcement ratio of the tension chord (= Ast /Act ) and db is the reinforcing bar diameter. Mid-way between the cracks, at z = s/2, the stresses are: σst2 =

T 2τ s − b As db

(3.51a)

σc2 =

2τb ρtc s db

(3.51b)

and

The maximum crack spacing immediately after loading, s = smax , occurs when σc2 = fct , and from Eq. 3.51b: smax =

fct db 2τb ρtc

(3.52)

with λ1 = 1.0 in Eq. 3.47. If the spacing between two adjacent cracks just exceeds smax , the concrete stress mid-way between the cracks will exceed fct and another crack will form between the two existing cracks. It follows that the minimum crack spacing is half the maximum value, that is, smin = smax /2. The instantaneous crack width (wi )tc in the ﬁctitious tension chord is the difference between the elongation of the tensile steel over the length s and the elongation of the concrete between the cracks and is given by: (wi )tc =

s T τ s − b (1 + nρtc ) Es Ast db

(3.53)

Depending on the dimensions of the cross-section and the concrete cover, the instantaneous crack width at the bottom concrete surface of the beam or slab, (wi )sofﬁt , may be different from that given by Eq. 3.53 for the tension chord and may be obtained from:

kcover s T τb s (wi )sofﬁt = kcover (wi )av = − (1 + nρtc ) Es Ast db

(3.54)

where kcover is a term to account for the dependence of crack width on the clear concrete cover c and may be taken as: kcover =

D − kd d − kd

5c (D − kd) − 2db

0.3 (3.55)

Design for serviceability

87

Under sustained load, additional cracks occur between widely spaced cracks (usually when 0.67smax < s ≤ smax ). The additional cracks are due to the combined effect of tensile creep rupture and shrinkage. As a consequence, the number of cracks increases and the maximum crack spacing reduces with time. The ﬁnal maximum crack spacing s∗ is only about two-thirds of that given by Eq. 3.52, but the ﬁnal minimum crack spacing remains about half of the value given by Eq. 3.52. As previously mentioned, experimental observations indicate that τb decreases with time, probably as a result of shrinkage-induced slip and tensile creep. Hence, the stress in the tensile concrete between the cracks gradually reduces. Furthermore, although creep and shrinkage will cause a small increase in the resultant tensile force T in the real beam and a slight reduction in the internal lever arm, this effect is relatively small and is ignored in the tension chord model presented here. The ﬁnal crack width is the elongation of the steel over the distance between the cracks minus the extension of the concrete caused by σcz plus the shortening of the concrete between the cracks due to shrinkage. For a ﬁnal maximum crack spacing of s∗ , the ﬁnal maximum crack width at the member sofﬁt is:

kcover s∗ T τb s∗ (w )sofﬁt = − (1 + ne ρtc ) − εsh Es Es Ast db ∗

(3.56)

where εsh is the shrinkage strain in the tensile concrete (and is a negative value); ne = Es /Ee = the effective modular ratio; Ee is the effective modulus given by Ee = Ec /(1 + ϕ(t, τ )); Ec and Es are the elastic moduli of the concrete and steel respectively; and ϕ(t, τ ) is the creep coefﬁcient of the concrete. A good estimate of the ﬁnal maximum crack width is given by Eq. 3.56, where s∗ is the maximum crack spacing after all time-dependent cracking has taken place, that is, s∗ = 0.67smax , and smax is given by Eq. 3.52. By rearranging Eq. 3.56, the steel stress on a cracked section corresponding to a particular maximum ﬁnal crack width (w∗ ) is given by: fst =

w ∗ Es τb s∗ + (1 + ne ρtc ) + εsh Es s∗ kcover db

(3.57)

By substituting τb (from Eq. 3.47) and s∗ = 0.67smax into Eq. 3.57 and by selecting a maximum desired crack width in a particular structure, w∗ , the maximum permissible tensile steel stress can be determined.

Example 3.6 The maximum ﬁnal crack widths determined using Eq. 3.56 are compared with the measured maximum ﬁnal crack widths for the 12 prismatic, oneway singly reinforced concrete specimens (six beams and six slabs) tested by Gilbert and Nejadi (Ref. 35). The specimens were described in Example 3.5 and their cross-sections are shown in Fig. 3.7 and details provided in Tables 3.9 and 3.10. Typical maximum crack width calculations are provided here for Beam B2-a.

88 Design for serviceability

Beam B2-a Relevant dimensions and properties are: b = 250 mm, D = 333 mm, d = 300 mm, Ast = 400 mm2 , Ec = 22,820 MPa, n = Es /Ec = 8.76, ϕ(t, τ ) = 1.71, εsh = −0.000825, Ee = 8420 MPa and ne = 23.8. A cracked section analysis gives kd = 78.8 mm and Icr = 212 × 106 mm4 . From Eq. 3.45, the area of concrete in the tension chord is Act = 0.5 × (333 − 78.8) × 250 = 31,780 mm2 and the reinforcement ratio of the tension chord ρtc = Ast /Act = 0.0126. When Ms = 24.8 kNm, the tensile force in the steel on the cracked section is Eq. 3.46: T=

8.76 × 24.8 × 106 (300 − 78.8) × 400 = 90.6 kN 212 × 106

and σst1 =

T = 226 MPa Ast

For short-term calculations, λ1 = 1.0 and, from Eqs 3.48 and 3.49, λ2 = 1.6 6˙ − 0.003˙ × 226 = 0.91 and λ3 = 7.0 − 0.3 × 16 = 2.2. With fct = 0.6 f c (t) = 2.57 MPa, the instantaneous bond stress is obtained from Eq. 3.47 as τb = 1.0 × 0.91 × 2.2 × 2.57 = 5.15 MPa and the maximum crack spacing immediately after loading is given by Eq. 3.52: smax =

2.57 × 16 = 317 mm 2 × 5.15 × 0.0126

For the calculation of the maximum ﬁnal crack width, the maximum crack spacing s∗ is taken as 2/3 of the instantaneous value and therefore s∗ = 2/3 × 317 = 211 mm. From Eq. 3.47, for long-term calculations, τb = 0.7 × 0.91 × 2.2 × 2.57 = 3.60 MPa and, from Eq. 3.55, kcover = 0.967. The maximum ﬁnal (long-term) crack width at the sofﬁt of the beam specimen B2-a is obtained from Eq. 3.56:

0.967 × 211 90,600 3.60 × 211 (w )sofﬁt = − (1 + 23.8 × 0.0126) 200,000 400 16 ∗

− (−0.000825) × 200,000 = 0.337 mm The measured maximum ﬁnal crack width on this specimen after 400 days under load was 0.36 mm. The measured and calculated maximum ﬁnal crack widths for all 12 test specimens are compared in Table 3.12. The mean of the ratios of predicted to measured crack widths for the six beam specimens is 1.059, with a coefﬁcient of variation of 22.8 per cent while for the six slab specimens the mean is 0.945, with a coefﬁcient of variation of 17.7 per cent. The agreement between the calculated and measured maximum ﬁnal crack width for this set of test data is good.

Design for serviceability Table 3.12 Comparison of measured and predicted maximum ﬁnal crack widths (mm) Specimen

B1-a

B1-b

B2-a

B2-b

B3-a

B3-b

S1-a

S1-b

S2-a

S2-b

S3-a

S3-b

Measured, wmax 0.38 0.18 0.36 0.18 0.28 0.13 0.25 0.20 0.23 0.18 0.20 0.15 Predicted, (w∗ )sofﬁt 0.425 0.262 0.337 0.207 0.212 0.122 0.287 0.196 0.258 0.155 0.162 0.111 1.119 1.457 0.935 1.149 0.758 0.936 1.148 0.981 1.123 0.863 0.812 0.742 (w∗ )sofﬁt /wmax

Example 3.7 A 150 mm thick simply-supported one-way slab located inside a building is to be considered. With appropriate regard for durability, the concrete strength is selected to be fc = 32 MPa and the cover to the tensile reinforcement is 20 mm. The ﬁnal shrinkage strain is taken to be εsh = −0.0006. Other relevant material properties are Ec = 28,600 MPa; n = Es /Ec = 7.0; ϕ(t, τ ) = 2.5; fct = 2.04 MPa and Es = 200 GPa. The effective modulus is therefore Ee = Ec /(1 + ϕ(t, τ )) = 8170 MPa and the effective modular ratio ne = Es /Ee = 24.5. The tensile face of the slab is to be exposed and the maximum ﬁnal crack width is to be limited to w∗ = 0.3 mm. After completing the design for strength and deﬂection control, the required minimum area of tensile steel is 650 mm2 /m. Under the full service loads, the maximum in-service sustained moment at mid-span is 20.0 kNm/m. The bar diameter and bar spacing must be determined so that the requirements for crack control are also satisﬁed.

Case 1 – Use 10 mm bars at 120 mm centres Ast = 655 mm2 /m at d = 125 mm and, referring to Figs 3.5 and 3.8, an elastic analysis of the cracked section gives kd = 29.6 mm and Icr = 50.3×106 mm4 . The maximum in-service tensile steel stress on the fully-cracked section at mid-span is calculated using Eq. 3.46 as σst1 = T/As = 265 MPa. The area of concrete in the tension chord is Act = 60,200 mm2 (Eq. 3.45) and the reinforcement ratio of the tension chord is ρtc = As /Act = 0.0109. From Eqs 3.48 and 3.49, λ2 = 0.78 and λ3 = 4.0 and from Eq. 3.47, τb = 6.39 MPa for short-term calculations (λ1 = 1.0) and τb = 4.47 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing s∗ is obtained using Eq. 3.52 as s∗ = 0.67smax = 97.6 mm and Eq. 3.55 gives kcover = 1.26. The maximum permissible steel stress required for crack control is obtained from Eq. 3.57: fst =

0.3 × 200,000 4.47 × 97.6 + (1 + 24.5 × 0.0109) 97.6 × 1.26 10 + (−0.0006 × 200,000) = 422 MPa

The actual stress at the crack σst = 265 MPa is much less than fst = 422 MPa and, therefore, cracking is easily controlled.

89

90 Design for serviceability

Case 2 – Use 12 mm bars at 170 mm centres As = 665 mm2 /m at d = 124 mm and, for this section, kd = 29.6 mm and Icr = 50.1 × 106 mm4 . The maximum in-service tensile steel stress on the fullycracked section at mid-span is σst1 = T/As = 264 MPa. The area of concrete in the tension chord is Act = 50,980 mm2 and ρtc = As /Act = 0.0130. Now λ2 = 0.79 and λ3 = 3.4 and τb = 5.47 MPa for shortterm calculations (λ1 = 1.0) and τb = 3.83 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing is s∗ = 114 mm and from Eq. 3.55, kcover = 1.29. The maximum permissible steel stress required for crack control is obtained from Eq. 3.57 as fst = 335 MPa – which is also signiﬁcantly greater than the actual maximum stress at the crack σst = 264 MPa. Therefore, the ﬁnal maximum crack width will be less than the maximum permissible value of 0.3 mm.

Case 3 – Use 16 mm bars at 300 mm centres As = 670 mm2 /m at d = 122 mm and, for this section, kd = 29.4 mm and Icr = 48.6 × 106 mm4 . The maximum in-service tensile steel stress on the fullycracked section at mid-span is σst1 = T/As = 266 MPa. The area of concrete in the tension chord is Act = 38,580 mm2 and ρtc = As /Act = 0.0174. Now λ2 = 0.78 and λ3 = 2.2 and τb = 3.50 MPa for short-term calculations (λ1 = 1.0) and τb = 2.45 MPa for long-term calculations (λ1 = 0.7). The maximum ﬁnal crack spacing is s∗ = 179 mm and from Eq. 3.55, kcover = 1.35. The maximum permissible steel stress required for crack control is fst = 167 MPa (from Eq. 3.57), which is much less than the actual steel stress due to the sustained moment of σst = 266 MPa. Therefore, crack control is not adequate and the maximum ﬁnal crack width will exceed 0.3 mm.

Simpliﬁed approaches – case 3 The deemed-to-comply crack control provisions of Eurocode 2 (2004) are in reasonable agreement with the above calculations, while the ACI 318-08 (Ref. 4) provisions are not. Considering ﬁrst the Eurocode 2 provisions, for case 3 above, the area of tensile steel provided exceeds the minimum steel area given by Eq. 3.42 and Table 3.7 suggests that, for a steel stress of σst1 = 266 MPa, if the maximum crack width is to be limited to 0.3 mm, the maximum bar diameter for crack control is 12 mm. Considering the ACI 318-08 requirement for Case 3, the area of tensile reinforcement exceeds the minimum value Ast.min given by Eq. 3.43, and with a steel stress of σst1 = 266 MPa, the maximum bar spacing permitted by Eq. 3.44 is 315 mm. With the bar spacing of 300 mm, Case 3 satisﬁes the requirements for crack control in ACI 318-08. The maximum crack widths predicted by the Gergely and Lutz expression (Eq. 3.35) and the two Eurocode 2 equations (Eqs 3.37 and 3.39) for case 3 are 0.284 mm, 0.304 mm and 0.244 mm, respectively. These indicate that the

Design for serviceability

91

maximum ﬁnal crack width will be less than (or in the case of Eurocode 2 (1992) only just greater than) the design crack width w∗ = 0.3 mm. In a structural design situation, all three approaches suggest that case 3 is acceptable. By contrast, the maximum crack width given by the equation proposed by Frosch (Eq. 3.36) is 0.528 mm, indicating that case 3 will lead to excessively wide cracks.

3.7.4 Model for direct tension cracking in restrained reinforced concrete Consider the fully restrained member shown in Fig. 3.10a (Refs 37 and 38). As the concrete shrinks, the restraining force N(t) gradually increases until the ﬁrst crack occurs when N(t) = Ac fct (t) (usually within a week of the commencement of shrinkage). At ﬁrst cracking, the restraining force reduces to Ncr , and the concrete stress away from the crack is less than the tensile strength of the concrete fct . The concrete on either side of the crack shortens elastically and the crack opens to a width w(t) that depends on the area of reinforcement (see Fig. 3.10b). At the crack, the steel carries the entire force Ncr and the stress in the concrete is clearly zero. In the region adjacent to the crack, the concrete and steel stresses vary considerably and the bond stress at the steel-concrete interface is high. At some distance so on each side of the crack, the concrete and steel stresses are no longer inﬂuenced directly by the presence of the crack, as shown in Figs 3.10c and 3.10d. Referring to Fig. 3.10, numerical values of Ncr , σc1 , σs1 , and σs2 can be obtained from (Ref. 37): Ncr =

nρfct Ac C1 + nρ(1 + C1 )

(3.58a)

σc1 =

Ncr (1 + C1 ) Ac

(3.58b)

σs1 = −C1 σs2 σs2 =

Ncr As

(3.58c) (3.58d)

where n is the modular ratio (Es /Ec ); ρ is the reinforcement ratio (As /Ac ); fct is the direct tensile strength of the concrete at ﬁrst cracking; and C1 =

2so 3L − 2so

(3.59)

The distance so in which stresses vary on either side of a crack depends on those factors that affect the bond stress at the steel concrete interface and include the reinforcement quantity, the bar diameter db and the surface characteristics of the bar. In Ref. 37 so was taken to be: so =

db 10ρ

(3.60)

92 Design for serviceability As = area of reinforcing steel Ac = area of concrete N(t)

N(t) (=Ac fct)

L

(a) Just prior to first cracking w Ncr

Ncr

L

(b) Just after first cracking so w so

sc1 Region 1

sc1 Region 2

Region 1

(c) Concrete stress just after first cracking ss2

ss1

so so w

ss1

(d) Steel stress just after first cracking

Figure 3.10 First cracking in a restrained direct tension member (Ref. 37).

This expression was used earlier by Favre et al. (Ref. 39) and others for a member containing deformed bars or welded wire mesh. Recent experimental results (Ref. 40) suggest that shrinkage causes a deterioration in bond at the steel-concrete interface and a gradual increase in so with time. For calculations at ﬁrst cracking (Eqs 3.58 and 3.59), so may be taken from Eq. 3.60, and for ﬁnal or long-term calculations, the value of so from Eq. 3.60 should be multiplied by 1.33 (Ref. 38) (i.e. (s∗o = 1.33 so ). The ﬁnal number of cracks and the ﬁnal average crack width depend on the length of the member, the quantity and distribution of reinforcement, the quality of bond between the concrete and steel, the amount of shrinkage and the concrete properties. In Fig. 3.11a, a portion of a restrained direct tension member is shown after all shrinkage has taken place and the ﬁnal crack pattern is established. The average concrete and steel stresses caused by shrinkage are illustrated in Figs 3.11bbreak and 3.11c. In many practical situations, the supports of a reinforced concrete member that provide the restraint to shrinkage are not immovable, but instead are adjacent parts of the structure that are themselves prone to shrinkage and other movements. If the supports of the restrained member in Fig. 3.10a suffer a relative movement u with time (in the direction of the length L), such that the ﬁnal length of the member is (L + u), the ﬁnal restraining force N(∞) changes and this affects both the crack

Design for serviceability w

w

93

w

s

s

(a) Portion of a restrained member after all cracking w

w

s*o s*o

s*o

w s*o

s*o

s *c1 Region 2

Region 1

s*o

s *c1 Region 2

Region 1

Region 2

(b) Concrete stress after all shrinkage cracking

s *s2

s *s2

s *s1

s *s2

s *s1

(c) Steel stress after all shrinkage cracking

Figure 3.11 Final concrete and steel stresses after direct tension cracking (Ref. 37).

spacing and the crack width. If u increases, N(∞) increases and so too does the number and width of the cracks. By enforcing the requirements of compatibility and equilibrium, expressions for the ﬁnal average crack spacing (s) and ﬁnal crack width (w) in a restrained member can be derived (Ref. 37). For a member containing m cracks and providing the reinforcing steel has not yielded, equating the overall elongation of the steel reinforcement to u gives:

∗ ∗ σ ∗ − σs1 σs1 2 ∗ L + m s2 (3.61) so + w = u Es Es 3 and, as w is much less than so , rearranging gives: ∗ σs1 =

−2 s∗o m ∗ 3 u Es σs2 + ∗ 3L − 2so m 3L − 2s∗o m

(3.62)

At each crack: ∗ σs2 = N(∞)/As

(3.63)

In Region 1 in Fig. 3.11, where the distance away from each crack exceeds s∗o (with taken as 1.33 times the value given by Eq. 3.60), the concrete stress history is shown diagrammatically in Fig. 3.12. The concrete tensile stress increases gradually with time as shrinkage progresses and approaches the direct tensile strength of the concrete fct . When cracking occurs elsewhere in the member, the tensile stress in the s∗o

94 Design for serviceability Concrete stress

fct sav sc1

s *c1

Time First cracking

Figure 3.12 Concrete stress history in uncracked Region 1 (Ref. 37).

uncracked regions drops suddenly as shown. Although the concrete stress history is continually changing, the average concrete stress at any time after the start of drying, σav , is between σc1 and fct , as shown in Fig. 3.12, and may be taken as the average of σc1 and fct (Ref. 37). The ﬁnal creep strain in Region 1 may be approximated by: εc∗ =

σav ∗ ϕ (τd ) Ec

(3.64)

where ϕ ∗ (τd ) is the ﬁnal creep coefﬁcient (at time inﬁnity) and τd is the age of the concrete when drying ﬁrst commenced. The ﬁnal concrete strain in Region 1 is the sum of the elastic, creep, and shrinkage components and may be approximated as: ∗ ε1∗ = εe + εc∗ + εsh =

σav σav ∗ ∗ + ϕ (τd ) + εsh Ec Ec

(3.65)

and the magnitude of the ﬁnal creep coefﬁcient ϕ ∗ (τd ) is usually between 2 and 4, depending on the age at the commencement of drying and the quality of the concrete. Eq. 3.65 may be expressed as: ε1∗ =

σav ∗ + εsh Ee

(3.66)

Ec ). 1 + φ ∗ (τd ) In Region 1, at any distance from a crack greater than so , equilibrium requires that the sum of the force in the concrete and the force in the steel is equal to N(∞). That is:

where Ee is the ﬁnal effective modulus for concrete (Ee =

∗ ∗ ∗ σc1 Ac + σs1 As = N(∞) or σc1 =

∗A N(∞) − σs1 s Ac

(3.67)

The compatibility requirement is that the ﬁnal concrete and steel strains are identical ∗ = ε ∗ ). Using Eq. 3.66, this becomes: (εs1 1 ∗ σs1 σav ∗ = + εsh Ee Es

(3.68)

Design for serviceability

95

Substituting Eqs 3.62 and 3.63 into Eq. 3.68 and rearranging gives: N(∞) =

3As Es u (3L − 2s∗o m)ne As ∗ Ee ) − (σav + εsh 2s∗o m 2s∗o m

(3.69)

With the restraining force N(∞) and the steel stress in Region 1 obtained from Eqs 3.69 and 3.62, respectively, the ﬁnal concrete stress in Region 1 is ∗ σc1 =

∗A N(∞) − σs1 s Ac

(3.70)

∗ ≤ f , where The number of cracks m is the lowest integer value of m for which σc1 ct the direct tensile strength fct should be taken as the mean 28-day value. The ﬁnal average crack spacing is s = L/m. The overall shortening of the concrete is an estimate of the sum of the crack widths. The ﬁnal concrete strain at any point in Region 1 of Fig. 3.11 is given by Eq. 3.66, and in Region 2, the ﬁnal concrete strain is:

ε2∗ =

∗ fnσc1 ∗ + εsh Ee

(3.71)

where fn varies between zero at a crack and unity at so from a crack. If a parabolic variation of stress is assumed in Region 2, the following expression for the average crack width w is obtained by integrating the concrete strain over the length of the member:

∗

σ 2 ∗ w = − c1 s − s∗o + εsh s (3.72) Ee 3 The preceding analysis is valid provided the assumption of linear-elastic behaviour in the steel is valid, that is, provided the steel has not yielded.

Example 3.8 The 140 mm thick slab of length 4 m shown in Fig. 3.13 is to be considered. The slab is rigidly held in position at each end support and, except for shrinkage, is unloaded. The slab is symmetrically reinforced with 12 mm diameter bars at 250 mm centres near both the top and bottom surfaces. Hence, As = 900 mm2 /m and ρ = As /Ac = 0.00643. The average ﬁnal spacing between the restrained shrinkage cracks and the average ﬁnal crack width are to be determined. D = 140 mm

L=4m

Figure 3.13 Slab of Example 3.8.

The material properties are: fc = 25 MPa; fct = 2.5 MPa; Ec = 25000 MPa; n = Es /Ec = 8.0; ϕ(t, τ ) = 3.0; E∗e = Ec /(1+ϕ ∗ (τ )) = 6250 MPa; ∗ ne = Es /E∗e = 32; and ∗ = −0.0007. εsh

96 Design for serviceability From Eqs 3.60 and 3.59: 12 = 187 mm and 10 × 0.00643 2 × 187 C1 = = 0.0321. 3 × 4000 − 2 × 187 so =

From Eqs 3.58a and b: Ncr =

8 × 0.00643 × 2.5 × 140,000 = 211 kN; 0.0321 + 8 × 0.00643 × (1 + 0.0321)

σc1 =

211,000 × (1 + 0.0321) = 1.55 MPa; 140,000

and therefore σav =

σc1 + fct = 2.02 MPa. 2

For ﬁnal shrinkage calculations: s∗o = 1.33 × 187 = 248 mm. The tabulation below shows the ﬁnal restraining force and concrete and steel stresses for different numbers of cracks: Number of cracks, m

N(∞) from Eq. 3.69 (kN)

∗ from σs1 Eq. 3.62 (MPa)

∗ from σs2 Eq. 3.63 (MPa)

∗ from σc1 Eq. 3.70 (MPa)

3 4 5 6

477 341 259 205

−75.1 −75.1 −75.1 −75.1

530 379 288 227

3.89 2.92 2.33 1.94

After the ﬁfth crack forms, the ﬁnal concrete stress is less than the tensile strength of concrete and the ﬁnal crack spacing is therefore about s = L/m = 800 mm. The ﬁnal crack width is estimated from Eq. 3.72:

2.33 2 w=− (800 − × 248) + (−0.0007 × 800) = 0.32 mm 6250 3

3.8 References 1. Sbarounis, J.A. (1984). Multi-storey ﬂat plate buildings – measured and computer one-year deﬂections. Concrete International, 6(8), 31–35. 2. Jokinen, E.P. and Scanlon, A. (1985). Field Measured Two-way Slab Deﬂections. CSCE Annual Conference, Saskatoon, Canada. 3. Gilbert, R.I. (1999). The risk and responsibility of structural engineers – A case study of a structural failure. International Congress – Creating with Concrete, University of Dundee, Scotland, Sept. Concrete Durability and Repair Technology, Thomas Telford, pp 773–783.

Design for serviceability

97

4. American Concrete Institute (2008), Building Code Requirements for Structural Concrete, ACI 318-08, Detroit. 5. British Standards Institution (1992). Eurocode 2: Design of Concrete Structures – Part 1: General rules and rules for buildings – DD ENV 1992-1-1:1992. European Committee for Standardization, Brussels. 6. British Standards Institution (2004). Eurocode 2: Design of Concrete Structures – part 1-1: General rules and rules for buildings – BS EN 1992-1-1:2004. European Committee for Standardization, Brussels. 7. Standards Australia (2009). Australian Standard for Concrete Structures, AS3600-2009. Sydney. 8. Standards Australia (2002). Structural design actions – Permanent, imposed and other actions AS/NZS 1170.1. Amendment 1: 2005, Amendment 2: 2009 (Australian/New Zealand Standards). 9. Standards Australia (2004). Bridge Design Part 2: Design Loads AS5100.2-2004. Sydney. 10. National Research Council of Canada (2005). National Building Code of Canada. Ottawa, Ontario. 11. British Standards Institution (1996). BS 6399: Part 1 – Loading for Buildings – Code of Practice for Dead and Imposed Loads. London. 12. American Association of State Highway and Transportation Ofﬁcials (2002). Standard Speciﬁcations for Highway Bridges AASHTO HB-17, Washington, DC. 13. American Society of Civil Engineers (2005). ASCE Standard ASCE 7-05 - Minimum Design Loads for Buildings and Other Structures. Reston, Virginia. 14. Standards Australia (2002). Structural design actions – Wind actions AS/NZS 1170.2. Amendment 1: 2005 (Australian/New Zealand Standards). 15. British Standards Institution (1997). BS 6399: Part 2 – Loading for Buildings – Code of Practice for Wind Loads. London. 16. Structural Engineers Association of California (2009). SEAOC Blue Book – Seismic Design Recommendations. Seismology Committee, Sacramento, CA. 17. Branson, D.E. (1965). Instantaneous and time-dependent deﬂections of simple and continuous reinforced concrete beams. HPR Report No. 7. Part 1. Alabama Highway Dept. Bureau of Public Roads, Alabama. 18. Gilbert, R.I. (2007). Tension stiffening in lightly reinforced concrete slabs. Journal of Structural Engineering, ASCE, 133(6), 899–903. 19. Irwin, A.W. (1978). Human response to dynamic motion of structures. The Structural Engineer, 56A(9). 20. Wilford, M. and Yound, P. (2006). A Design Guide for Footfall induced Vibrations of Structures. The Concrete Centre, Camberley, UK. 21. Mayer, H. and Rüsch, H. (1967). Building Damage Caused by Deﬂection of Reinforced Concrete Building Components. Technical Translation 1412, National Research Council Ottawa, Canada (Deutscher Auschuss für Stahlbeton, Heft 193, Berlin, West Germany, 1967). 22. Rangan, B.V. (1982). Control of beam deﬂections by allowable span-depth ratios. ACI Journal, 79(5), 372–377. 23. Gilbert, R.I. (1985). Deﬂection control of slabs using allowable span to depth ratios. ACI Journal, 82(1), 67–72. 24. The Concrete Society (2005). Deﬂections in concrete slabs and beams. Technical Report No. 58. 25. Bischoff, P.H. (2005). Reevaluation of deﬂection prediction for concrete beams reinforced with steel and FRP bars. Journal of Structural Engineering, ASCE, 131(5), 752–767. 26. Gilbert, R.I. (1999). Deﬂection calculations for reinforced concrete structures – why we sometimes get it wrong. ACI Structural Journal, 96(6), 1027–1032.

98 Design for serviceability 27. Patrick, M. (2009). Beam deﬂection by simpliﬁed calculation: including effect of compressive reinforcement in formula for σcs in draft AS3600. BD-002 Committee Document. 28. Gilbert R.I. (2003). Deﬂection by simpliﬁed calculation in AS3600-2001 – on the determination of fcs . Australian Journal of Structural Engineering, Engineers Australia, 5(1), 61–71. 29. Gilbert, R.I. (2008). Instantaneous and time-dependent deﬂection of reinforced concrete ﬂexural members. Concrete Forum – Journal of the Concrete Institute of Australia, 1(1), 7–17. 30. Gilbert, R.I. (2001). Deﬂection calculation and control – Australian code amendments and improvements. In ACI International SP 203, Code Provisions for Deﬂection Control in Concrete Structures, Chapter 4, American Concrete Institute. Editors E.G. Nawy and A. Scanlon, Detroit, 45–78. 31. Gergely, P. and Lutz, L.A. (1968). Maximum crack width in reinforced concrete ﬂexural members. In Causes, Mechanism, and Control of Cracking in Concrete, SP-20, American Concrete Institute, Farmington Hills, MI, 1–17. 32. Frosch, R.J. (1999). Another look at cracking and crack control in reinforced concrete. ACI Structural Journal, 96(3), 437–442. 33. Marti, P., Alvarez, M., Kaufmann, W. and Sigrist, V. (1998). Tension chord model for structural concrete. Structural Engineering International, 4/98, 287–298. 34. Gilbert, R.I. (2008). Control of ﬂexural cracking in reinforced concrete. ACI Structural Journal, 105(3), 301–307. 35. Gilbert, R.I. and Nejadi, S. (2004). An Experimental Study of Flexural Cracking in Reinforced Concrete Members under Sustained Loads. UNICIV Report No. R-435, School of Civil and Environmental Engineering, University of New South Wales, Sydney, Australia. 36. Wu, H.Q. and Gilbert, R.I. (2009). Modelling short-term tension stiffening in reinforced concrete prisms using a continuum-based ﬁnite element model. Engineering Structures, 31(10), 2380–2391. 37. Gilbert, R.I. (1992). Shrinkage cracking in fully-restrained concrete members. ACI Structural Journal, 89(2), 141–149. 38. Nejadi, S. and Gilbert, R.I. (2004). Shrinkage cracking and crack control in restrained reinforced concrete members. ACI Structural Journal, 101(6), 840–845. 39. Favre, R. et al. (1983). Fissuration et Deformations. Manual du Comite Euro-International du Beton (CEB), Ecole Polytechnique Federale de Lausanne, Switzerland. 40. Nejadi, S. and Gilbert, R.I. (2004). Shrinkage Cracking in Restrained Reinforced Concrete Members. UNICIV Report No. R-433, School of Civil and Environmental Engineering, The University of New South Wales, Sydney, Australia.

4

Uncracked sections Axial loading

4.1 Preamble In the previous chapter, simpliﬁed methods were presented for the determination of deﬂection and crack widths. While often suitable for design purposes, the simpliﬁed methods approximate structural deformation at service loads without necessarily providing an insight into the time-dependent behaviour of the structure. In situations where accurate and reliable estimates of the effects of creep and shrinkage are required, the simpliﬁed methods of Chapter 3 may not be adequate. More reﬁned methods are available that realistically model the time-dependent deformation of concrete structures and also enable the calculation of the redistribution of stresses between the concrete and the reinforcement and the redistribution of internal actions in statically indeterminate members. Reﬁned methods for the time analysis of cross-sections are introduced in this chapter and illustrated using the simple example of a symmetrically reinforced cross-section subjected to a constant sustained axial compressive load. The time analysis of a concrete structure involves the determination of strains, stresses, curvatures and deﬂections at critical points and at critical times during the life of the structure. Often a structural designer is most interested in the ﬁnal deformation and the ﬁnal internal actions at time inﬁnity after the effects of creep and shrinkage have taken place, i.e. the long-term behaviour. The creep and shrinkage characteristics of concrete are highly variable and are never known exactly. In addition, the methods for the time analysis of concrete structures are plagued by simplifying assumptions and approximations. Accurate numerical predictions of time-dependent behaviour are therefore not possible. However, it is possible, and indeed necessary, to establish upper and lower limits to the ﬁnal stresses and deformations in order to determine whether or not time effects are critical in any particular situation and, if required, to adjust the design in order to reduce undesirable long-term deformations. If the concrete stress σc (τ0 ) at a point in a structure, ﬁrst applied at age τ0 , remains constant with time, each of the concrete strain components may be calculated readily as follows: ε (t) = εe (t) + εcr (t) + εsh (t) =

σc (τ0 ) σc (τ0 ) + ϕ(t, τ0 ) + εsh (t) Ec (τ0 ) Ec (τ0 )

(4.1)

Numerical values of ϕ(t, τ0 ) and εsh (t) may be obtained from the models discussed in Sections 2.1.4 and 2.1.5, and the calculation of time-dependent structural behaviour is relatively straightforward.

100 Uncracked sections If the concrete stress at a point varies with time, the determination of the creep strain becomes more involved. In reinforced concrete structures, even under constant sustained loads, stresses are rarely constant and Eq. 4.1 can no longer be used to predict deformation accurately. The stress history and the effects of ageing must be included. In this chapter, several methods for the time analysis of cross-sections are discussed and applied to a simple practical problem. The mathematical description of each procedure is followed by a discussion of its strengths and weaknesses, and its advantages and disadvantages. To illustrate each procedure, the analysis of a symmetrically reinforced concrete column section under a constant axial compressive load is presented and numerical results obtained using each procedure are compared.

4.2 The effective modulus method 4.2.1 Formulation The simplest and oldest technique for including creep in structural analysis is Faber’s effective modulus method (EMM) (Ref. 1). In Section 1.2.4, the instantaneous and creep components of strain were combined and a reduced or effective modulus for concrete, Ee (t, τ0 ), was deﬁned in Eqs 1.11 and 1.12. In Section 1.2.5, the integraltype creep law was presented in Eq. 1.17 to describe the time-dependent deformation of a continuously varying stress history. In the EMM, Eq. 1.17 is approximated by assuming that the stress-dependent deformations are produced only by a sustained stress equal to the ﬁnal value of the stress history, that is: t ε(t) = τ0

=

1 + ϕ (t, τ ) 1 + ϕ (t, τ0 ) dσc (τ ) + εsh (t) ≈ σc (t) + εsh (t) Ec (τ ) Ec (τ0 )

σc (t) + εsh (t) Ee (t, τ0 )

(4.2)

where Ee (t, τ0 ) is the effective modulus for concrete deﬁned in Eq. 1.12 (which for convenience is repeated here) as: Ee (t,τ0 ) =

Ec (τ0 ) 1 + ϕ(t,τ0 )

(4.3)

Creep is treated as a delayed elastic strain and is taken into account simply by reducing the elastic modulus of concrete with time. A time analysis using the effective modulus method is nothing more than an elastic analysis in which Ee (t, τ0 ) is used instead of Ec (τ0 ). Shrinkage may be included in this elastic time analysis in a similar way as a sudden temperature change in the concrete would be included in a short-term elastic analysis. According to the EMM, the creep strain at time t (in Eq. 4.2) depends only on the current stress in the concrete σc (t) and is therefore independent of the previous stress history. This, of course, is not the case. The ageing of the concrete has been ignored. For an increasing stress history, the EMM overestimates creep, while for a decreasing

Uncracked sections 101 stress history, creep is underestimated. If the stress is entirely removed, the creep strains disappear. The EMM therefore predicts complete creep recovery, which is not correct. Eq. 4.2 is valid only when the concrete stress is constant in time. In such cases, the EMM gives excellent results. Good results are also obtained if the concrete is old when ﬁrst loaded and the effect of ageing is not great. Despite its shortcomings, the EMM is the simplest of all of the methods for the time analysis of concrete structures and its simplicity recommends it, particularly under the conditions mentioned above. In many practical problems, the method is sufﬁciently accurate for design purposes. However, many practical situations involve rapidly changing stress histories in young concrete. In such cases, the EMM may be unsuitable and potentially misleading, and a more sophisticated method of analysis is required. 4.2.2 Example application (EMM) Consider the short, axially-loaded, symmetrically reinforced column shown in Fig. 4.1. The column is subjected to a constant, sustained axial force P as shown. Creep and shrinkage cause a gradually decreasing stress history in the concrete similar to that shown in Fig. 1.15. The redistribution of internal forces due to the gradual development of creep and shrinkage strains is to be examined and the time-dependent stresses and strains in both the concrete and the steel are to be calculated using the EMM. The problem is solved by enforcing the three basic requirements of any time analysis: namely, equilibrium of forces, compatibility of strains and satisfaction of the constitutive relationships of the concrete and the steel. The external compressive load P is applied at time τ0 and is resisted by the internal forces in the concrete and steel Nc (t) and Ns (t), where at any time t after loading Nc (t) = σc (t)Ac and Ns (t) = σs (t)As . Equilibrium requires that the sum of the internal forces at time t equals the external load, that is: P = Nc (t) + Ns (t) = σc (t)Ac + σs (t)As

P

(4.4)

P P = constant

Ac L Nc(t) Ns(t)

(a) Elevation

As

(b) Section

Figure 4.1 Axially-loaded short column.

102 Uncracked sections Compatibility requires that the total concrete strain ε(t) and the steel strain εs (t) are identical at all times: ε(t) = εs (t)

(4.5)

The concrete constitutive relationship used in the EMM is given by Eq. 4.2 and the steel is assumed to be linear and elastic, with modulus Es . Therefore, at any time t: ε(t) =

σc (t) + εsh (t) Ee (t, τ0 )

(4.6a)

and σs (t) Es

εs (t) =

(4.6b)

Re-arranging Eqs 4.6 in terms of σc (t) and σs (t) gives: σc (t) = ε(t)Ee (t, τ0 ) − εsh (t)Ee (t, τ0 )

(4.7a)

σs (t) = εs (t)Es

(4.7b)

and

Inserting these equations into the equilibrium equation (Eq. 4.4) and enforcing compatibility (Eq. 4.5) yields: P = Ee (t, τ0 )ε(t)Ac − Ee (t, τ0 )εsh (t)Ac + ε(t)Es As

(4.8)

which represents the governing equation of the problem. Solving Eq. 4.8 for the unknown total concrete strain ε(t) gives: ε(t) = =

P Ac Ee (t, τ0 )εsh (t) + Ac Ee (t, τ0 ) + As Es Ac Ee (t, τ0 ) + As Es P ε (t) + sh Ac Ee (t, τ0 )(1 + ne ρ) 1 + ne ρ

(4.9)

where ne = the effective modular ratio = Es /Ee (t, τ0 ) and ρ = the reinforcement ratio = As /Ac . By substituting Eq. 4.9 into Eq. 4.7a, the concrete stress at time t is obtained: σc (t) =

P Es ρ εsh (t) − Ac (1 + ne ρ) 1 + ne ρ

(4.10)

The steel strain εs (t) is identical to the total concrete strain ε(t) (Eq. 4.5) and therefore the steel stress may be obtained by substituting Eq. 4.9 into Eq. 4.7b: σs (t) =

ne P Es εsh (t) + Ac (1 + ne ρ) 1 + ne ρ

(4.11a)

Uncracked sections 103 The steel stress may also be obtained from the equilibrium equation (Eq. 4.4): σs (t) =

P − σc (t)Ac As

(4.11b)

The elastic component of concrete strain at time t is usually taken to be εe (t) = σc (t)/Ec (τ0 ) and the creep strain is therefore εcr (t) = ε(t) − εe (t) − εsh (t).

Example 4.1 Consider the short, symmetrically reinforced column shown in Fig. 4.1. The column is subjected to a constant sustained axial force P = −1000 kN ﬁrst applied at age τ0 = 14 days. The cross-sectional areas of the concrete and the steel reinforcement are Ac = 90,000 mm2 and As = 1800 mm2 , respectively, and the reinforcement ratio is therefore ρ = As /Ac = 0.02. The column is located in a temperate environment and shrinkage is assumed to commence at the age of ﬁrst loading. The mean in-situ compressive strength of concrete at the time of ﬁrst loading is taken to be fcmi (τ0 ) = 28 MPa and the characteristic 28-day compressive strength is fc = 40 MPa. The elastic modulus of concrete at ﬁrst loading is Ec (τ0 ) = 26.7 GPa and the elastic modulus of steel is Es = 200 GPa. The creep coefﬁcient is obtained from Eq. 2.3 and shrinkage strain is obtained ∗ = −510×10−6 . from Eq. 2.6, with ﬁnal (long-term) values: ϕ ∗ (τ0 ) = 2.39 and εsh The variations of the creep coefﬁcient and shrinkage with time are given in the following table and shown in Fig. 4.2. For illustrative purposes it has been assumed that shrinkage begins at the time of loading. (t − τ0 ) in days

0

10

30

70

200

500

10,000

ϕ(t, τ0 ) εsh (t − τ0 ) × 10−6

0 0

0.53 −142

0.98 −246

1.38 −325

1.83 −407

2.10 −456

2.39 −510

Creep coefficient

2.5 2 1.5 1 0.5 0 0

200

400

600

Time, t (days)

800

1000

Shrinkage strain (× −10−6)

The redistribution of internal forces due to the gradual development of creep and shrinkage strains is to be examined and the time-dependent changes in stresses and strains in both the concrete and the steel are to be calculated. Sample calculations are provided below. 600 500 400 300 200 100 0 0

200

400

600

800

1000

Time, t (days)

Figure 4.2 Creep coefﬁcient and shrinkage strain versus time curves for Example 4.1.

104 Uncracked sections

At ﬁrst loading τ0 , (t − τ0 ) = 0: ϕ(t, τ0 ) = 0 and εsh (t − τ0 ) = 0. With Ee (t, τ0 ) = Ec (τ0 ) = 26.7 GPa; and ne = n = Es /Ec (τ0 ) = 7.48. Eq. 4.9: Eq. 4.5:

ε(τ0 ) =

−1000 × 103 + 0 = −361 × 10−6 ; 90,000 × 26,700 × (1 + 7.48 × 0.02)

εs (τ0 ) = −361 × 10−6 ;

Eq. 4.7a:

σc (τ0 ) = −361 × 10−6 × 26,700 − 0 = −9.67 MPa;

Eq. 4.7b:

σs (τ0 ) = −361 × 10−6 × 200,000 = −72.3 MPa.

The stresses in the concrete and steel could have also been calculated directly from Eqs 4.10 and 4.11: Eq. 4.10:

σc (τ0 ) =

−1000 × 103 − 0 = −9.67 MPa; 90,000(1 + 7.48 × 0.02)

Eq. 4.11b:

σs (τ0 ) =

−1000 × 103 + 9.67 × 90,000 = −72.3 MPa. 1800

With the creep and shrinkage components of the concrete strain both equal to zero at ﬁrst loading, the concrete strain ε(τ0 ) is entirely made up of the elastic or instantaneous component of strain εe (τ0 ).

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + ϕ(t, τ0 )) = 17.48 GPa; and ne = Es /Ee (t, τ0 ) = 11.44; and Eq. 4.9:

ε(t) =

−1000 × 103 −142 × 10−6 + 90,000 × 17,480 × (1 + 11.44 × 0.02) 1 + 11.44 × 0.02

= −633 × 10−6 ; Eq. 4.5: Eq. 4.7a:

εs (t) = −633 × 10−6 ; σc (t) = −633 × 10−6 × 17,480 − (−142 × 10−6 ) × 17,480 = −8.58 MPa;

Eq. 4.7b:

σs (t) = −633 × 10−6 × 200,000 = −126.6 MPa.

The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −321 × 10−6 ; the shrinkage component of strain is εsh (t) = −142 × 10−6 ; and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −170 × 10−6 .

Uncracked sections 105 The results of the analyses at ﬁrst loading and throughout the period of sustained loading are provided in the following table. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) −9.67 −8.58 −7.82 −7.23 −6.66 −6.35 −6.02

0 10 30 70 200 500 10,000

Steel stress σs (t) (MPa) −72.3 −127 −165 −194 −222 −238 −255

Total Elastic Creep Shrinkage strain concrete strain strain ε(t) strain εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −633 −824 −969 −1112 −1191 −1273

−361 −321 −292 −270 −249 −237 −225

0 −170 −285 −374 −456 −497 −538

0 −142 −246 −325 −407 −456 −510

4.3 The principle of superposition – step-by-step method (SSM) 4.3.1 Formulation The principle of superposition and its applicability for the determination of strains in concrete was discussed in Section 1.2.5. The creep strain produced by a stress increment applied at any time τi is assumed to be unaffected by any other stress increment applied either earlier or later. The superposition integral for the total concrete strain at any time t due to a time-varying stress history (Eq. 1.17) cannot be solved in closed form unless simplifying assumptions are made, such as the parallel creep curve assumption illustrated subsequently in Fig. 4.10. In the step-by-step method (SSM), a solution technique is employed using the incremental form of the superposition equation (Eq. 1.16). The period of sustained stress is divided into k time intervals as shown in Fig. 4.3, with the age at ﬁrst loading designated τ0 and the end of the period of sustained stress designated τk . Consider the time-varying stress history shown in Fig. 4.4. The actual stress history is approximated by a step-wise variation of stress, with an increment of stress σc (τj ) applied at the end of each time interval, as shown. For this decreasing stress history, if the initial stress σc (τ0 ) is compressive, the stress increments σc (τj ) applied at the end of each time interval are tensile. The stress is assumed to remain constant during Concrete pour t0 t 1

t2

tj

tk-1

First loading

tk

Time, t

End of time period

Figure 4.3 Time discretisation.

106 Uncracked sections Stress sc(t0)

sc(t) Dsc(tj)

j-th time interval, Dtj

t 0 t1 t 2

tj−1

tj

tk Time

Figure 4.4 Time-varying stress history – SSM.

each time interval. The greater the number of time intervals, the more accurate is the ﬁnal prediction. Various formulations of the SSM are available in the literature (for example, Refs 2–5), all of which give similar answers provided the time intervals are suitably small. For a particular time interval τk − τ0 , the time discretisation should be such that an approximately equal portion of the creep coefﬁcient ϕ(τk , τ0 ) develops during each time step. A convenient and effective time discretisation based on a geometrical progression is given by: (τk − τ0 ) τk k 1/(k−1) τj = τ0 + τk k τj−1 − τ0 τ1 = τ0 +

(4.12a) (4.12b)

where τ0 and τk deﬁne the beginning and end of the time period to be discretised; k represents the number of time intervals; and j = 2, 3, . . ., k. The SSM is perfectly general and can be used to predict behaviour due to any stress or strain history using any desired creep and shrinkage curves. Using the integral in the integral-type creep law (Eq. 1.17): t ε(t) = J (t, τ0 )σc (τ0 ) +

J (t, τ )dσc (τ ) + εsh (t)

τ0+

and the total concrete strain at the end of the j-th time period (t = τj ) may be approximated by:

ε(τj ) = J (τj , τ0 )σc (τ0 ) +

j J τj , τi σc (τi ) + εsh (τj )

(4.13a)

i=1

where J(τj , τi ) represents the creep (compliance) function calculated at time τj related to a unit stress applied at time τi , while σc (τi ) is calculated as σc (τi )−σc (τi−1 ) and depicts the stress variation that occurs between times τi−1 and τi . A better approximation is

Uncracked sections 107 obtained if the average creep function associated with the time step τi and τi−1 is used within the summation in Eq. 4.13a, that is: j J τj , τi + J τj , τi−1 σc (τi ) + εsh (τj ) ε(τj ) = J (τj , τ0 )σc (τ0 ) + 2

(4.13b)

i=1

Eq. 4.13a approximates the integral-type creep law by means of the so-called rectangular rule, while Eq. 4.13b represents the trapezoidal rule. Both approximations tend towards the same result as the number of time steps increases. Simplifying the notation, Eqs 4.13a and 4.13b become, respectively: εj − εsh,j = Jj,0 σc,0 +

j

Jj,i σc,i

(4.13c)

i=1

and εj − εsh,j = Jj,0 σc,0 +

j Jj,i + Jj,i−1

2

i=1

σc,i

(4.13d)

where εj = ε(τj ); εsh,j = εsh (τj ); Jj,0 = J (τj , τ0 ); σc,0 = σc (τ0 ); Jj,i = J τj , τi ; σc,i = σc (τi ) and σc (τi ) = σc,i − σc,i−1 . Eqs 4.13a and b can be expressed in terms of creep coefﬁcients as follows: j

ε(τj ) =

1 + ϕ (τj , τi ) 1 + ϕ (τj , τ0 ) σc (τ0 ) + σc (τi ) + εsh (τj ) Ec (τ0 ) Ec (τi )

(4.14a)

i=1

and

j 1+ϕ (τj ,τ0 ) 1 1+ϕ (τj ,τi ) 1+ϕ (τj ,τi−1 ) σc (τ0 )+ + σc (τi )+εsh (τj ) ε(τj ) = Ec (τ0 ) 2 Ec (τi ) Ec (τi−1 ) i=1

(4.14b) Simplifying the notation gives: j

εj − εsh,j =

1 + ϕj,i 1 + ϕj,0 σc,0 + σc,i Ec,0 Ec,i

(4.14c)

i=1

and j

1 1 + ϕj,0 σc,0 + εj − εsh,j = Ec,0 2 i=1

1 + ϕj,i−1 1 + ϕj,i + Ec,i Ec,i−1

σc,i

where ϕj,0 = ϕ(τj , τ0 ), ϕj,i = ϕ (τj , τi ), Ec,0 = Ec (τ0 ) and Ec,i = Ec (τi ).

(4.14d)

108 Uncracked sections As Eqs 4.14 indicate, a large amount of input data is required for the SSM. For each time step, Ec (τi ) and ϕ(τj , τi ) must be speciﬁed and the previous stress history must be stored throughout the analysis. However, the SSM is not subject to many of the simplifying assumptions contained in other methods of analysis and generally leads to reliable results. For most practical problems, satisfactory results are obtained using as few as 6–10 time intervals. For illustrative purposes, Eqs 4.13a and 4.14a are used in the following. The axially loaded, symmetrically reinforced column shown in Fig. 4.1, and analysed in Section 4.2.2, is re-analysed here using the SSM. Time is discretised into a preselected number of time intervals. Two approaches will be considered: (i) Approach 1 obtains the solution by calculating the change in concrete stress that occurs at the end of each time step; and (ii) Approach 2 expresses the governing system of equations in terms of the concrete stress at the time considered. Both approaches are in fact identical and differ only in the manipulation of the governing equations. 4.3.2 Example application (SSM) – Approach 1 In Approach 1, Eq. 4.14a is used to calculate the change in stress at the end of each time step. For the continuously varying stress history shown in Fig. 4.4, the stress increment, σc (τi ), is assumed to be applied at the end of the i-th time interval, as shown. The increments of instantaneous plus creep strain caused by σc (τi ) are calculated at the end of each time interval using the appropriate elastic modulus and creep coefﬁcient (Ec (τi ) and ϕ(τj , τi ), respectively). The total strain at the end of each time interval is obtained by superposition of the strain increments caused by stress changes in all previous time intervals and by shrinkage. 4.3.2.1 At ﬁrst loading (t = τ0 ) Following the approach outlined in Section 4.2.2 for the EMM, the instantaneous stresses and strains at τ0 immediately after the application of the axial force P, and before any creep and shrinkage has occurred, are obtained using Eqs 4.5–4.11 and are given by: ε(τ0 ) =

P ; εs (τ0 ) = ε(τ0 );σc (τ0 ) = ε(τ0 )Ec (τ0 ); and σs (τ0 ) = εs (τ0 )Es Ac Ec (τ0 )(1+n0 ρ)

where n0 = Es /Ec (τ0 ) = the modular ratio at time τ0 and ρ = As /Ac = the reinforcement ratio. The analysis at each subsequent time step is outlined in the following. 4.3.2.2 At the end of the j-th time step (i.e. t = τj ) The stress in the concrete at the end of the j-th time step is: σc (τj ) = σc (τj−1 ) + σc (τj )

(4.15)

Uncracked sections 109 where σc (τj−1 ) is known as it has been calculated at the previous time step and σc (τj ) is the unknown stress increment at τj . The equilibrium and compatibility equations are:

σc (τj−1 ) + σc (τj ) Ac + σs (τj ) As = P

(4.16)

and ε(τj ) = εs (τj )

(4.17)

The stress–strain relationships for the concrete and the steel at time τj are: j

ε(τj ) =

1 + ϕ (τj , τi ) 1 + ϕ (τj , τ0 ) σc (τ0 ) + σc (τi ) + εsh (τj ) Ec (τ0 ) Ec (τi )

(4.18a)

i=1

and εs (τj ) =

σs (τj ) Es

(4.18b)

Rearranging Eqs 4.18 in terms of stresses at time τj gives: j−1 Ec (τj ) σc (τi ) σc (τ0 ) − Ec (τj ) − Ec (τj )εsh (τj ) σc τj = Ec (τj )ε(τj ) − Ee (τj , τ0 ) Ee (τj , τi ) i=1

(4.19a) and σs τj = Es εs (τj )

(4.19b)

where Ee (τj , τi ) is the effective modulus of concrete at time τj associated with a stress increment ﬁrst applied at time τi and is given by: Ee (τj , τi ) =

Ec (τi ) 1 + ϕ (τj , τi )

(4.20)

By substituting Eqs 4.19 and 4.17 into Eq. 4.16 and simplifying, the unknown strain, ε(τk ), is readily determined as: ⎤ ⎡ j−1 σc (τj−1 ) ne,j,0 σc (τ0 ) ne,j,i σc (τi ) 1 P ⎣ + + εsh (τj )⎦ − + ε(τj ) = 1 + nj ρ Ac Ec (τj ) Ec (τj ) Es Es i=1

(4.21)

110 Uncracked sections where nj = Es /Ec (τj ) = the modular ratio at time τj ; ne,j,0 = Es /Ee (τj , τ0 ) and ne,j,i = Es /Ee (τj , τi ) are the effective modular ratios; and ρ = the reinforcement ratio = As /Ac . The steel strain εs (τj ) is found using Eq. 4.17 and is identical to the total concrete strain ε(τj ). The concrete stress increment is obtained from Eq. 4.19a: ⎡ σc (τj ) =

1 ⎣ P − σc (τj−1 ) − ne,j,0 ρσc (τ0 ) − 1 + nj ρ Ac

j−1

⎤ ne,j,i ρσc (τi ) − εsh (τj )Es ρ ⎦

i=1

(4.22) With σ (τj ) calculated from Eq. 4.22, the concrete stress at τj is obtained from Eq. 4.15. The steel stress σs (τj ) is determined from Eq. 4.19b. Alternatively, σs (τj ) could also be calculated from the equilibrium equation (Eq. 4.16). From the strain calculated at time instant τj (ε(τj ) = εs (τj )), the axial deformation or axial shortening of the column can be readily calculated. For the column of length, L, shown in Fig. 4.1, the axial shortening of the column at time, τj , due to the applied load, P, and shrinkage is designated eL (τj ) and given by: eL (τj ) = Lε(τj )

(4.23)

The approach is useful in the determination of time-dependent axial shortening in the columns and walls of multi-storey buildings where differential shortening may be an important design consideration.

Example 4.2 The symmetrically reinforced column analysed in Example 4.1 (refer Fig. 4.1) is to be re-analysed here using the SSM. As in the previous example, the column is subjected to an axial load P = −1000 kN ﬁrst applied at age τ0 = 14 days and then held constant. The properties of the column cross-section are: Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; and Es = 200 GPa. In this example, the six time intervals speciﬁed in the following table are considered for illustrative purposes. A signiﬁcant amount of input data is required; speciﬁcally, a different creep coefﬁcient and elastic modulus for each concrete stress increment applied at the end of each time interval. The following table contains the input data necessary to obtain the concrete and steel stresses and strains at the end of each time interval. The concrete properties are obtained from the material modelling procedures outlined in Chapter 2, that is, Ec (τj ) from Eqs 2.2a and 2.2c, ϕ(τj , τi ) from Eq. 2.3 and εsh (τj ) from Eq. 2.6. The concrete is mixed with high early strength cement. As in Example 4.1, shrinkage is taken to begin at the time of ﬁrst loading.

Uncracked sections 111 j

0

1

2

3

4

5

6

τj (days)

14

24

44

84

214

514

10,014

t − τj (days)

0

10

30

70

200

500

10,000

ϕ(τj , τ0 ) ϕ(τj , τ1 ) ϕ(τj , τ2 ) ϕ(τj , τ3 ) ϕ(τj , τ4 ) ϕ(τj , τ5 )

0

0.53 0

0.98 0.72 0

1.38 1.18 0.90 0

1.83 1.63 1.44 1.22 0

2.10 1.89 1.69 1.51 1.26 0

2.39 2.15 1.94 1.75 1.54 1.38

Ec (τj ) (MPa)

26,700

27,900

28,900

29,700

30,500

31,000

31,700

εsh (τj ) × 10−6

0

−142

−246

−325

−407

−456

−510

Note that the shrinkage strains and the creep coefﬁcients associated with the age at ﬁrst loading, τ0 , are the same as those adopted previously in Example 4.1 using the EMM. The family of creep coefﬁcient versus the logarithm of time curves is shown in Fig. 4.5. 3

Creep coefficient

2.5 2 1.5 1 0.5

j(t,t0)

0

14

j(t,t2) j(t,t1)

24

44

10

j(t,t3) j(t,t4)

84 100

214

j(t,t5)

514 1000

10,000

Time (days) (log scale)

Figure 4.5 Creep coefﬁcient versus log time curves for Example 4.2.

At ﬁrst loading (τ0 ): As in Example 4.1, with Ec (τ0 ) = Ee (τ0 , τ0 ) = 26.7 GPa and n0 = Es /Ec (τ0 ) = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε(τ0 ) = −361 × 10−6 ; εs (τ0 ) = −361 × 10−6 ; σc (τ0 ) = −9.67 MPa and σs (τ0 ) = −72.3 MPa.

At time instant τ1 = 24 days (time step 1 from τ0 to τ1 ): For time interval, j = 1: Ec (τ0 ) = 26.7 GPa; Ec (τ1 ) = 27.9 GPa; n1 = Es /Ec (τ1 ) = 7.17; ϕ(τ1 , τ0 ) = 0.53; Ee (τ1 , τ0 ) = Ec (τ0 )/(1 + ϕ(τ1 , τ0 )) = 17.48 GPa; ne,1,0 = Es /Ee (τ1 , τ0 ) = 11.44; and εsh (τ1 ) = −142 × 10−6 .

112 Uncracked sections From Eq. 4.22:

1 −1000 × 103 σc (τ1 ) = + 9.67 + 11.44 × 0.02 × 9.67 1 + 7.17 × 0.02 90,000 + 142 × 10−6 × 200,000 × 0.02 = 1.17 MPa

The concrete stress at τ1 is therefore σc (τ1 ) = σc (τ0 ) + σc (τ1 ) = −9.67 + 1.17 = −8.50 MPa −1000 × 103 + 8.50 × 90,000 = −131 MPa 1800 Eq. 4.18b and Eq. 4.17 give: and from Eq. 4.16: σs (τ1 ) =

εs (τ1 ) =

−131 = −653 × 10−6 200,000

ε(τ1 ) = −653 × 10−6 At time τ1 , the elastic component of the concrete strain is εe (τ1 ) = σc (τ0 )/Ec (τ0 )+ σ (τ1 )/Ec (τ1 ) = −319 × 10−6 ; the shrinkage component of strain is εsh (τ1 ) = −142 × 10−6 ; and therefore the creep component of strain is εcr (τ1 ) = ε(τ1 ) − εe (τ1 ) − εsh (τ1 ) = −192 × 10−6 .

At time instant τ2 = 44 days (time step 2 from τ1 to τ2 ): Time interval, j= 2: Ec (τ0 ) = 26.7 GPa; Ec (τ1 ) = 27.9 GPa; Ec (τ2 ) = 28.9 GPa; n2 = Es /Ec (τ2 ) = 6.92; ϕ(τ2 , τ0 ) = 0.98; Ee (τ2 , τ0 ) = Ec (τ0 )/(1 + ϕ(τ2 , τ0 )) = 13.53 GPa; ne,2,0 = Es /Ee (τ2 , τ0 ) = 14.78; ϕ(τ2 , τ1 ) = 0.72; Ee (τ2 , τ1 ) = Ec (τ1 )/(1 + ϕ(τ2 , τ1 )) = 16.25 GPa; ne,2,1 = Es /Ee (τ2 , τ1 ) = 12.31; εsh (τ2 ) = −246 × 10−6 . Eq. 4.22: 1 −1000×103 σ (τ2 ) = +8.50+14.78×0.02× 1+6.92×0.02 90,000 ×9.67 −12.31×0.02×1.17 +246×10

−6

×200,000×0.02

= 0.83 MPa The concrete stress at τ2 is therefore: σc (τ2 ) = σc (τ1 ) + σc (τ2 ) = −8.50 + 0.83 = −7.67 MPa

Uncracked sections 113 and from Eq. 4.16, the steel stress is: σs (τ2 ) =

−1000 × 103 + 7.67 × 90,000 = −172 MPa 1800

The steel strain is obtained from Eq. 4.18b and the total concrete strain from Eq. 4.17: εs (τ2 ) =

−172 = −860 × 10−6 200,000

and ε (τ2 ) = −860 × 10−6 At time τ2 , the elastic component of concrete strain is: εe (τ2 ) = σc (τ0 )/Ec (τ0 ) + σc (τ1 )/Ec (τ1 ) + σc (τ2 )/Ec (τ2 ) = −291 × 10−6 ; the shrinkage component is εsh (τ2 ) = −246 × 10−6 ; and therefore the creep component of strain is: εcr (τ2 ) = ε(τ2 ) − εe (τ2 ) − εsh (τ2 ) = −323 × 10−6 .

At subsequent time instants Similarly, the stress and strain components at the end of each subsequent time step are calculated and the results are tabulated below. Instant Time τj Concrete Concrete Steel Total Elastic Creep Shrinkage j (days) stress stress stress strain strain strain strain increment σc (τj ) σs (τj ) ε(τj ) εe (τj ) εcr (τj ) εsh (τj ) σc (τj ) (MPa) (MPa) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) (MPa) 0 1 2 3 4 5 6

14 24 44 84 214 514 10,014

– 1.17 0.83 0.63 0.65 0.34 0.41

−9.67 −8.50 −7.67 −7.04 −6.39 −6.05 −5.64

−72.3 −131 −172 −204 −236 −253 −273

−361 −653 −860 −1018 −1180 −1264 −1367

−361 −319 −291 −269 −248 −237 −225

0 −192 −323 −424 −525 −571 −632

0 −142 −246 −325 −407 −456 −510

The effect of increasing the number of time steps on the accuracy of the predictions using the SSM is illustrated below. In the following table, the results of further analyses are presented in which the time discretisation proposed in Eqs 4.12 has been adopted. Either 6 or 18 time steps have been considered between τ0 and each of the previously considered time instants (τk in the ﬁrst

114 Uncracked sections column of the table below). The results provided on each line of the table have been produced by separate time analyses using the SSM. Time τk (days)

14 24 44 84 214 514 10,014

No of time steps used

Concrete stress σc (τk ) (MPa)

Steel stress (MPa)

Total strain ε(τk ) (×10−6 )

Elastic strain εe (τk ) (×10−6 )

Creep strain εcr (τk ) (×10−6 )

Shrinkage strain εsh (τk ) (×10−6 )

1 6 (18) 6 (18) 6 (18) 6 (18) 6 (18) 6 (18)

−9.67 −8.54 (−8.55) −7.68 (−7.72) −7.02 (−7.09) −6.36 (−6.46) −6.00 (−6.10) −5.65 (−5.71)

−72.3 −129 (−128) −171 (−169) −205 (−201) −238 (−233) −255 (−251) −273 (−270)

−361 −644 (−641) −857 (−847) −1023 (−1006) −1188 (−1164) −1277 (−1253) −1366 (−1349)

−361 −320 (−320) −291 (−292) −269 (−270) −247 (−249) −236 (−238) −225 (−226)

0 −182 (−179) −320 (−309) −430 (−411) −534 (−508) −586 (−559) −631 (−613)

0 −142 (−142) −246 (−246) −325 (−325) −407 (−407) −456 (−456) −510 (−510)

Based on these results, increasing the number of time steps by a factor of three has produced changes in the ﬁnal total strain and in the ﬁnal concrete and steel stresses of less than 2 per cent. Considering the uncertainty associated with the estimates of the concrete properties, there is little to be gained, from a practical point of view, by considering more than about 6–10 time steps in most situations. The axial shortening of the column is calculated using Eq. 4.23. If the overall length of the column is 4000 mm, the column shortening at ﬁrst loading and after 10,000 days are eL (τ0 = 14) = 1.44 mm and eL (τ18 = 10,014) = 5.40 mm, respectively. The axial shortening of the column has increased with time by a factor of almost four.

4.3.3 Example application (SSM) – Approach 2 In approach 2, the concrete constitutive relationship is manipulated so that the concrete stress at the end of each time instant is obtained directly. If the rectangular approximation of the integral-type creep law is used, Eq. 4.13c may be rearranged as follows: εj − εsh,j = Jj,0 σc,0 +

j

Jj,i σc,i

i=1 j−1

= Jj,0 σc,0 + Jj,j σc,j − σc,j−1 + Jj,i σc,i − σc,i−1 i=1

= Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 +

j−1 i=1

Jj,i σc,i −

j−1 i=1

Jj,i σc,i−1

Uncracked sections 115 j−1

= Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 +

i=1

j−2

Jj,i σc,i −

Jj,i+1 σc,i

i=0

j−2 = Jj,0 σc,0 + Jj,j σc,j − Jj,j σc,j−1 + Jj,j−1 σc,j−1 + Jj,i − Jj,i+1 σc,i − Jj,1 σc,0 i=1 j−1

= Jj,0 σc,0 + Jj,j σc,j +

Jj,i − Jj,i+1 σc,i − Jj,1 σc,0 i=1 j−1

Jj,i − Jj,i+1 σc,i = Jj,j σc,j + Jj,0 − Jj,1 σc,0 + i=1

and therefore: j−1 Jj,i − Jj,i+1 σc,i εj − εsh,j = Jj,j σc,j +

(4.24)

i=0

Expressing Eq. 4.24 in terms of the stress at the end of the j-th time step, the constitutive relationship for the concrete at any time τj becomes: σc,j =

εj − εsh,j Jj,j

−

j−1 Jj,i − Jj,i+1 i=0

Jj,j

j−1

σc,i

= Ec,j εj − εsh,j + Fe,j,i σc,i

(4.25)

i=0

where Ec,j is the instantaneous elastic modulus of concrete at τj ; Fe,j,i is the stress modiﬁcation factor; and these terms are deﬁned as Ec,j =

1 Jj,j

(4.26a)

and Fe,j,i =

Jj,i+1 − Jj,i Jj,j

(4.26b)

For completeness, the corresponding expressions for Ec,j and Fe,j,i to be used in Eq. 4.25 when adopting the trapezoidal approximation of the integral-type creep law are: For i = 0: 1 Ec,j = (4.26c) Jj,j and Fe,j,i =

Jj,1 − Jj,0 Jj,j + Jj,j−1

(4.26d)

For i > 0: Ec,j =

2 Jj,j + Jj,j−1

(4.26e)

116 Uncracked sections and Fe,j,i =

Jj,i+1 − Jj,i−1 Jj,j + Jj,j−1

(4.26f)

Noting that the steel and concrete strains are always identical, the equilibrium equation at the end of the j-th time step for the axially loaded column example can be expressed as: P = σc,j Ac + σs,j As = Ac Ec,j εj − Ac Ec,j εsh,j +

j−1

Ac Fe,j,i σc,i + As Es εj

(4.27)

i=0

where σs,j = σs (τj ) and εj (= εs,j ) is the strain in both the concrete and the steel at τj . Solving for the concrete strain εj gives: j−1

εj =

Ac Ec,j εsh,j Ac Fe,j,i P + − σc,i Ac Ec,j + As Es Ac Ec,j + As Es Ac Ec,j + As Es

(4.28)

i=0

and observing that Ac Ec,j = Ac Ec,j + As Es

1 1 = Es As 1 + nj ρ 1+ Ec,j Ac

Eq. 4.28 can be rewritten as: ⎞ ⎛ j−1 Fe,j,i 1 ⎝ P εj = + εsh,j − σc,i ⎠ 1 + nj ρ Ac Ec,j Ec,j

(4.29)

i=0

It is also noted that: Jj,i+1 − Jj,i Fe,j,i 1 1 1 1 − = = Jj,j = Jj,i+1 − Jj,i = − Ec,j Jj,j Ee,j,i+1 Ee,j,i Ee τj , τi+1 Ee τ j , τ i =

ne,j,i+1 ne,j,i − Es Es

where ne,j,i = Es /Ee,j,i and, for ease of notation, Ee,j,i = Ee (τj , τi ). Eq. 4.29 can therefore be simpliﬁed to: ⎞ ⎛ j−1 ne,j,i+1 − ne,j,i 1 ⎝ P + εsh,j − σc,i ⎠ εj = 1 + nj ρ Ac Ec,j Es i=0

(4.30)

Uncracked sections 117 Substituting Eq. 4.30 into Eq. 4.25 gives: ⎞ ⎛ j−1 j−1 ne,j,i+1 −ne,j,i 1 ⎝P ⎠ +Ec,j εsh,j −Ec,j σc,i −Ec,j εsh,j + Fe,j,i σc,i σc,j = 1+nj ρ Ac Es i=0

=

i=0

j−1

ne,j,i+1 −ne,j,i 1 P −nj ρ Ec,j εsh,j −Ec,j σc,i 1+nj ρ Ac Es i=0

+

j−1

Fe,j,i σc,i +nj ρ

i=0

j−1

Fe,j,i σc,i

i=0

which can be simpliﬁed to: ⎡ ⎤ j−1 1 ⎣P − Es ρ εsh,j + ρ ne,j,i+1 − ne,j,i σc,i ⎦ σc,j = 1 + nj ρ Ac

(4.31)

i=0

With the concrete stress σc,j at time, τj , calculated from Eq. 4.31, the steel stress is obtained from the equilibrium equation: σs,j =

P − σc,j Ac As

(4.32)

and the steel and concrete strains are obtained from Eqs 4.18b and 4.17, respectively.

Example 4.3 The column analysed in Example 4.2 is to be re-analysed here using approach 2. As before, P = −1000 kN; Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; Es = 200 GPa and the time varying concrete properties are: j

0

1

2

3

4

5

6

τj (days)

14

24

44

84

214

514

10,014

t − τj (days)

0

10

30

70

200

500

10,000

ϕ(τj , τ0 ) ϕ(τj , τ1 ) ϕ(τj , τ2 ) ϕ(τj , τ3 ) ϕ(τj , τ4 ) ϕ(τj , τ5 )

0

0.53 0

0.98 0.72 0

1.38 1.18 0.90 0

1.83 1.63 1.44 1.22 0

2.10 1.89 1.69 1.51 1.26 0

2.39 2.15 1.94 1.75 1.54 1.38

Ec (τj ) (MPa) εsh (τj ) × 10−6

26,700 27,900 28,900 29,700 30,500 31,000 31,700 0

−142

−246

−325

−407

−456

−510

118 Uncracked sections

At ﬁrst loading (τ0 ): As in Example 4.2, with Ec,0 = Ee,0 = 26.7 GPa; and n0 = Es /Ec,0 = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε0 = −361×10−6 ; εs,0 = −361×10−6 ; σc,0 = −9.67 MPa and σs,0 = −72.3 MPa.

At time instant τ1 = 24 days (time step 1 from τ0 to τ1 ): For time interval, j = 1: Ec,0 = 26.7 GPa; Ec,1 = 27.9 GPa; n1 = Es /Ec,1 = 7.17; ϕ1,0 = 0.53; Ee,1,0 = Ec,0 /(1 + ϕ1,0 ) = 17.48 GPa; ne,1,0 = Es /Ee,1,0 = 11.44; ne,1,1 = Es /Ee,1,1 = 7.17 and εsh,1 = −142 × 10−6 . From Eq. 4.31, the concrete stress at the end of the ﬁrst time step (j = 1) is: 1 −1000 × 103 σc,1 = − 200,000 × 0.02 × (−142 × 10−6 ) 1 + 7.17 × 0.02 90,000 + 0.02 × (7.17 − 11.44) × (−9.67) = −8.50 MPa. −1000 × 103 + 8.50 × 90,000 = −131 MPa; 1800 −131 Eq. 4.18b and Eq. 4.17 give: εs,1 = = −653 × 10−6 and ε1 = 200,000 −653 × 10−6 . As calculated in Example 4.2, the elastic, creep and shrinkage components of the concrete strain at time τ1 are εe,1 = −319 × 10−6 , εcr,1 = −192 × 10−6 , and εsh (τ1 ) = −142 × 10−6 . and from Eq. 4.32: σs,1 =

At time instant τ2 = 44 days (time step 2 from τ1 to τ2 ): Time interval, j = 2: Ec,0 = 26.7 GPa; Ec,1 = 27.9 GPa; Ec,2 = 28.9 GPa; n2 = Es /Ec,2 = 6.92; ϕ2,0 = 0.98; Ee,2,0 = Ec,0 /(1 + ϕ2,0 ) = 13.53 GPa; ne,2,0 = Es /Ee,2,0 = 14.78; ϕ.2,1 = 0.72; Ee,2,1 = Ec,1 /(1+ϕ2,1 ) = 16.25 GPa; ne,2,1 = Es /Ee,2,1 = 12.31; and εsh,2 = −246 × 10−6 . From Eq. 4.31, the concrete stress at the end of the ﬁrst time step (j = 1) is: 1 −1000 × 103 σc,2 = − 200,000 × 0.02 × (−246 × 10−6 ) 1 + 6.92 × 0.02 90,000 +0.02 × [(12.31 − 14.78) × (−9.67) + (6.92 − 12.31) × (−8.50)] = −7.67 MPa and from Eq. 4.32: σs,1 =

−1000 × 103 + 7.67 × 90,000 = −172 MPa. 1800

Uncracked sections 119 Eqs 4.18b and 4.17 give: εs,1 =

−172 = −860 × 10−6 and ε1 = 200,000

−860 × 10−6 . As in Example 2.2, the elastic, creep and shrinkage components of concrete strain at τ2 are εe,2 = −291 × 10−6 ; εcr,2 = −323 × 10−6 , and εsh (τ2 ) = −246 × 10−6 .

At subsequent time instants: Similarly, the stress and strain components at the end of each subsequent time step are calculated and the results are tabulated below. It can be seen that the results obtained using the SSM with approaches 1 and 2 are identical. Instant Time τj Concrete Steel Total Elastic Creep Shrinkage j (days) stress stress strain strain strain strain σc (τj ) σs (τj ) ε(τj ) εe (τj ) εcr (τj ) εsh (τj ) (MPa) (MPa) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) 0 1 2 3 4 5 6

14 24 44 84 214 514 10,014

−9.67 −8.50 −7.67 −7.04 −6.39 −6.05 −5.64

−72.3 −131 −172 −204 −236 −253 −273

−361 −653 −860 −1018 −1180 −1264 −1367

−361 −319 −291 −269 −248 −237 −225

0 −192 −323 −424 −525 −571 −632

0 −142 −246 −325 −407 −456 −510

4.4 The age-adjusted effective modulus method (AEMM) 4.4.1 Formulation A simple adjustment to the effective modulus method to account for the ageing of concrete was proposed by Trost (Ref. 6). Later the method was more rigorously formulated and further developed by Dilger and Neville (Ref. 7) and Bazant (Ref. 8). The method is sometimes called the Trost–Bazant Method (Ref. 9), but Bazant’s more descriptive title, the age-adjusted effective modulus method, is preferred here. Consider the two concrete stress histories and the corresponding creep-time curves shown in Fig. 4.6. In stress history (a), σc (τ0 ) is applied at time τ0 and subsequently held constant with time. In stress history (b), the stress σc (t) is gradually applied, beginning at τ0 and reaching a magnitude equal to σc (τ0 ) at time τk . The creep strain at any time t(> τ0 ) produced by the gradually applied stress σc (t) is signiﬁcantly smaller than that resulting from the stress σc (τ0 ) abruptly applied at τ0 , as shown. This is due to ageing. The earlier a concrete specimen is loaded, the greater the ﬁnal creep strain. A reduced creep coefﬁcient can therefore be used to calculate creep strain if stress is gradually applied. Let this reduced creep coefﬁcient be χ(t, τ0 )ϕ(t, τ0 ), where the coefﬁcient χ (t, τ0 ) is called the ageing coefﬁcient (< 1.0).

120 Uncracked sections Stress (a) Constant stress

Creep strain

ecr.a(tk,t0) ecr.b(tk,t0)

sc(t0)

(b) Gradually applied stress t0

Time, t

ecr.a(tk,t0) =

tk

t0

tk

Time, t

sc(t0) s (t ) j(tk ,t0) ; ecr.b(tk,t0) = 0 0 c(tk ,t0)j(tk ,t0) Ec(t0) Ec(t0)

Figure 4.6 Creep due to constant and variable stress histories.

The creep strain at time, t, due to a stress, σc (t), that has been gradually applied over the time interval t − τ0 , may be expressed as: εcr (t) =

σc (t) χ(t, τ0 ) ϕ(t, τ0 ) Ec (τ0 )

(4.33)

The magnitude of the ageing coefﬁcient χ (t, τ0 ) generally falls within the range 0.4 to 1.0 depending on the rate of application of the gradually applied stress in the period after τ0 . Consider the gradually reducing stress history shown in Fig. 4.7. An initial compressive stress σc (τ0 ) applied at time τ0 is reduced with time due to the application of a gradually increasing tensile stress increment σc (t). The change of stress may be due to a change of the external loads, or restraint to creep and shrinkage, or variations of temperature, or combinations of these, and is usually unknown at the beginning of an analysis. Using the AEMM, the total strain at time t may be expressed as the sum of the strains produced by σc (τ0 ) (instantaneous and creep), the strains produced by the

Stress

sc(t) = sc(t0)+ Dsc(t)

sc(t0) Dsc(t)

sc(t) t0

t

Figure 4.7 A gradually reducing stress history.

Time

Uncracked sections 121 gradually applied stress increment σc (t) (instantaneous and creep), and the shrinkage strain: ε(t) = =

σc (τ0 ) σc (t) [1 + ϕ(t,τ0 )] + [1 + χ(t, τ0 ) ϕ(t, τ0 )] + εsh (t) Ec (τ0 ) Ec (τ0 ) σc (τ0 ) σc (t) + εsh (t) + Ee (t, τ0 ) Ee (t, τ0 )

(4.34)

where Ee (t, τ0 ) is the effective modulus of Eq. 4.3 and Ee (t, τ0 ) is the age-adjusted effective modulus given by: Ee (t, τ0 ) =

Ec (τ0 ) 1 + χ(t, τ0 ) ϕ(t, τ0 )

(4.35)

With the AEMM, two analyses need to be carried out: one at ﬁrst loading (time τ0 ) and one at time t after the period of sustained stress. Unlike the EMM, the ﬁnal strain depends on the stress at ﬁrst loading σc (τ0 ) and the change in stress that occurs with time σc (t). The reinforced concrete column shown in Fig. 4.1 is to be analysed using the AEMM. As for the SSM, two approaches will also be considered here: (i) Approach 1 obtains the solution for the concrete stress at time t, σc (t), by calculating the change in stress that occurs over the entire period of sustained loading, σc (t); and (ii) Approach 2 calculated the stress at time t, σc (t), directly. Both approaches lead to the same solution and differ only in the manipulation of the governing equations. 4.4.2 Example application (AEMM) – Approach 1 The instantaneous analysis at time τ0 (immediately after the application of the axial force P, and before any creep and shrinkage has occurred) is identical to that presented earlier and the instantaneous stresses and strains are: σc (τ0 ) =

P P − σc (τ0 )Ac σc (τ0 ) σs (τ0 ) ; ε(τ0 ) = ; σs (τ0 ) = and εs (τ0 ) = Ac (1 + n0 ρ) As Ec (τ0 ) Es

where n0 = Es /Ec (τ0 ) = the modular ratio at time τ0 and ρ = As /Ac = the reinforcement ratio. As described in Section 4.2.2, the equilibrium and compatibility requirements at any time t are speciﬁed by Eqs 4.4 and 4.5, respectively: P = σc (t)Ac + σs (t)As

(4.4)

εs (t) = ε(t)

(4.5)

and

122 Uncracked sections The constitutive relationship for concrete is described by Eq. 4.34 and, as before, the steel is linear-elastic: ε(t) =

σc (τ0 ) σc (t) + εsh (t) + Ee (t, τ0 ) Ee (t, τ0 )

(4.36a)

and εs (t) =

σs (t) Es

(4.36b)

where σc (t) is the unknown time-dependent change of stress caused by creep and shrinkage. If σc (τ0 ) is compressive, the stress increment σc (t) is usually tensile. Rearranging Eqs 4.36 in terms of time-varying stresses gives: σc (t) = Ee (t, τ0 )ε(t) −

Ee (t, τ0 ) Ee (t, τ0 )εsh (t) σc (τ0 ) − Ee (t, τ0 )

(4.37a)

and σs (t) = Es εs (t)

(4.37b)

At any time, t, the concrete stress is given by: σc (t) = σc (τ0 ) + σc (t)

(4.38)

and the governing equation of the problem is obtained by substituting Eqs 4.37, 4.38 and 4.5 into Eq. 4.4 and solving for the unknown total strain ε(t): ε (t) =

1 P 1 1 + σc (τ0 ) + εsh (t) − 1 + n¯ e,0 ρ Ee (t, τ0 )Ac Ee (t, τ0 ) Ee (t, τ0 )

(4.39)

where ne,0 = Es /Ee (t, τ0 ), ρ = As /Ac , and n¯ e,0 = Es / Ee (t, τ0 ) = the age-adjusted modular ratio. By substituting Eq. 4.39 into Eq. 4.36a, the concrete stress increment σc (t) can be expressed as:

1 P σc (t) = − σc (τ0 )(1 + ne,0 ρ) − εsh (t) Es ρ 1 + n¯ e,0 ρ Ac

(4.40)

With σc (t) calculated from Eq. 4.40, the resultant steel and concrete stresses at time t are given by Eqs 4.37b and 4.38. Alternatively, these could be calculated from equilibrium considerations (Eq. 4.4). 4.4.3 Determination of the ageing coefﬁcient Numerical values for χ (t, τ0 ) can be obtained from the associated creep coefﬁcient ϕ(t, τ0 ) if the stress change σc (t) is known. Like the creep coefﬁcient, the ageing

Uncracked sections 123 coefﬁcient χ (t, τ0 ) depends on the age of the concrete at ﬁrst loading τ0 , the duration of load (t − τ0 ), the size and shape of the member, and so on. For the gradually decreasing concrete stress history when a member is subjected to a constant sustained load, the ageing coefﬁcient χ (t, τ0 ) may be obtained by rearranging and expanding Eq. 4.40. With shrinkage set to zero, χ (t, τ0 ) is given by: χ (t, τ0 ) =

σc (τ0 ) 1 1 + nρ − σc (τ0 ) − σc (t) ϕ (t, τ0 ) nρ

(4.41)

If the stress history of Fig. 4.7 is the result of pure relaxation (i.e. when the member is restrained and the strain ε(t) remains constant with time at its initial value of σc (τ0 )/Ec (τ0 )), the ageing coefﬁcient χ (t, τ0 ) may be obtained by rearranging the expanded form of Eq. 4.34: χ (t, τ0 ) =

σc (τ0 ) 1 − σc (τ0 ) − σc (t) ϕ (t, τ0 )

(4.42a)

Eq. 4.42a is commonly expressed in the literature in the following form: χ (t, τ0 ) =

Ec (τ0 ) 1 − Ec (τ0 ) − R (t, τ0 ) ϕ (t, τ0 )

(4.42b)

in which R(t, τ0 ) represents the relaxation function deﬁned as the stress at time t due to a unit strain applied at time τ0 and kept constant throughout the period τ0 to t. Values for R(t, τ0 ) can be readily calculated by applying the SSM (Eq. 4.25) to the case of a constant unit strain history beginning at τ0 . Using a step-by-step numerical analysis (Section 4.3.2) to establish the gradual loss of concrete stress with time (σc (t) = σc (t) − σc (τ0 )), ageing coefﬁcients χ (t, τ0 ) may be readily determined for the creep coefﬁcients ϕ(t, τ0 ) speciﬁed by Eq. 2.3 in Section 2.1.4. For the cross-section, concrete properties and loading details of Examples 4.1 and 4.2, the ageing coefﬁcients associated with the gradual concrete stress change under a constant external load P ﬁrst applied at age τ0 are calculated using Eq. 4.41 and shown in Fig. 4.8. Also shown in Fig. 4.8 are the ageing coefﬁcients calculated using Eq. 4.42a associated with the more rapid change in concrete stress caused by pure relaxation (i.e. when the total strain ε(t) is held constant with time and the applied load P varies as a result of relaxation). Neville et al. (Ref. 9) and others have shown that ageing coefﬁcients calculated in this way, when used in conjunction with the age-adjusted effective modulus method, provided close agreement with experimental data. Fig. 4.9 shows the variation with time of the ageing coefﬁcients obtained from the creep coefﬁcients of Eq. 2.3 for a creep problem similar to that of Examples 4.1 and 4.2. For concrete loaded in the ﬁrst few weeks after casting (such as for the curves corresponding to τ0 = 7 and 14 days in Fig. 4.9), and for load durations exceeding about 100 days, the ageing coefﬁcient is between 0.55 and 0.72 for normal strength concrete with a value of 0.65 being suitable for most practical situations where ﬁnal deformations are required. Considering how uncertain are the predictions of ϕ(t, τ0 )

124 Uncracked sections

Ageing coefficient

0.9 Constant deformation (relaxation problem)

0.8 0.7

Constant load, P (creep problem)

0.6 0.5 0.4 100

10

1000

10,000

Time after loading in days (log scale)

Figure 4.8 Ageing coefﬁcient versus time for the concrete used in Example 4.2. 1

t0 = 7 days Ageing coefficient

Ageing coefficient

1 0.9 f ʹc

Eq. 4.42 0.8

25 MPa 40 MPa

0.7 25 MPa

0.6 0.5

60 MPa 40 MPa

60 MPa

25 MPa

0.8

40 MPa 25 MPa

0.7 0.6

60 MPa 40 MPa

Eq. 4.41

t0 = 14 days

0.4 10

100

1000

10,000

10

Eq. 4.42

0.8

60 MPa

0.7 Eq. 4.41 0.6 0.5

t0 = 28 days

0.4 10

100

1000

Time after loading in days (log scale)

1000

10,000

1

f ʹc 25 MPa 40 MPa 60 MPa 25 MPa 40 MPa

Ageing coefficient

1

100

Time after loading in days (log scale)

Time after loading in days (log scale)

0.9

60 MPa

0.5

Eq. 4.41

0.4

Ageing coefficient

f ʹc

Eq. 4.42

0.9

10,000

Eq. 4.42

0.9 0.8

25 MPa

40 MPa

0.7

60 MPa f ʹc

Eq. 4.41

0.6 0.5

t0 = 100 days

0.4 10

100

1000

10,000

Time after loading in days (log scale)

Figure 4.9 Ageing coefﬁcients versus time derived from ϕ(t, τ0 ) taken from Eq. 2.3 (with th = 150 mm and interior environment).

and the other concrete properties, the following values of the ﬁnal ageing coefﬁcient are recommended for use in structural design: For concrete loaded at early ages τ0 < 20 days: χ (∞, τ0 ) = χ ∗ (τ0 ) = 0.65 for creep problems (constant load)

(4.43a)

χ(∞, τ0 ) = χ ∗ (τ0 ) = 0.80 for relaxation problems (constant deformation) (4.43b)

Uncracked sections 125 For concrete loaded at later ages τ0 > 28 days: χ (∞, τ0 ) = χ ∗ (τ0 ) = 0.75 for creep problems

(4.43c)

χ(∞, τ0 ) = χ ∗ (τ0 ) = 0.85 for relaxation problems

(4.43d)

The use of Eq. 4.43 simpliﬁes the age-adjusted effective modulus method and usually leads to good approximations of both material and structural behaviour. The inadequacies of the effective modulus method are to a large extent overcome by the introduction of the ageing coefﬁcient. Bazant (Ref. 8) pointed out that the method is theoretically exact for any problem in which strain varies proportionally with the creep coefﬁcient (provided, of course, the ageing coefﬁcient has been carefully calculated from the assumed creep coefﬁcient). Extracting χ(t, τ0 ) from Fig. 4.9 is not particularly suitable for computer application nor is it generally necessary. The approximations of Eq. 4.43 are suitable for most applications.

Example 4.4 The symmetrically reinforced column analysed in Example 4.1 (see Fig. 4.1) under a constant sustained axial load P is re-analysed here using the AEMM. As before: P = −1000 kN, Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02 and Es = 200 GPa. The variation of the creep coefﬁcient and shrinkage with time were given in Example 4.1 and, for convenience, are repeated in the following table. The ageing coefﬁcients are taken from Fig. 4.9 and are also given below. All other data as given in Example 4.1. (t − τ0 ) in days

0

10

30

70

200

500

10,000 (∞)

ϕ(t, τ0 ) χ (t, τ0 ) εsh (t − τ0 ) × 10−6

0 – 0

0.53 0.60 −142

0.98 0.64 −246

1.38 0.67 −325

1.83 0.70 −407

2.10 0.70 −456

2.39 0.69 −510

At ﬁrst loading, (t − τ0 ) = 0: ϕ(t, τ0 ) = 0 and εsh (τ0 ) = 0. As in Example 4.1: with Ec (τ0 ) = Ee (τ0 ) = 26.7 GPa; and n0 = Es /Ec (τ0 ) = 7.48, the instantaneous stresses and strains immediately after ﬁrst loading are: ε(τ0 ) = −361 × 10−6 ; εs (τ0 ) = −361 × 10−6 ; σc (τ0 ) = −9.67 MPa and σs (τ0 ) = −72.3 MPa.

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53, χ (t, τ0 ) = 0.60 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + ϕ(t, τ0 )) = 17.48 GPa; and ne,0 = Es /Ee (t, τ0 ) = 11.44; Ee (t, τ0 ) = Ec (τ0 )/(1 + χ (t, τ0 )ϕ(t, τ0 )) = 20.27 GPa; and n¯ e,0 = Es / Ee (t, τ0 ) = 9.87.

126 Uncracked sections Eq. 4.40:

1 −1000×103 σc (t) = +9.67(1+11.44×0.02) 1+9.87 ×0.02 90,000 +142×10−6 ×200,000×0.02 = +1.12 MPa;

Eq. 4.38: Eq. 4.4: Eq. 4.36b: Eq. 4.5:

σc (t) = −9.67 +1.12 = −8.55 MPa; σs (t) = ((−1000×103 +8.55×90,000)/1800 = −128.0 MPa; εs (t) = −128.0/200,000 = −640×10−6 ; and ε(t) = −640×10−6 .

The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −320 × 10−6 and εsh (t) = −142 × 10−6 ; and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −178 × 10−6 . The results of the analyses at ﬁrst loading and throughout the period of sustained loading are provided in the following table. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) 0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.48 −6.12 −5.73

Steel stress σs (t) (MPa) −72.3 −128 −169 −200 −232 −249 −269

Total Elastic Creep Shrinkage strain strain strain strain ε(t) εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −640 −843 −1002 −1158 −1247 −1346

−361 −320 −289 −266 −242 −229 −214

0 −178 −308 −411 −509 −563 −622

0 −142 −246 −325 −407 −456 −510

By comparison, the variations of stresses and strains in this example if the approximation of Eq. 4.43 is adopted throughout (i.e. if χ (t, τ0 ) is equal to 0.65 for all values of t) are provided below. For practical purposes, the two sets of results are the same. Time t (days)

14 24 44 84 214 514 10,014

Duration Concrete of load stress t − τ0 σc (t) (days) (MPa) 0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.45 −6.08 −5.69

Steel stress σs (t) (MPa) −72.3 −128 −169 −201 −233 −252 −271

Total Elastic Creep Shrinkage strain strain strain strain ε(t) εe (t) εcr (t) εsh (t) (×10−6 ) (×10−6 ) (×10−6 ) (×10−6 ) −361 −639 −843 −1004 −1166 −1258 −1355

−361 −320 −289 −265 −241 −227 −213

0 −177 −307 −413 −518 −575 −632

0 −142 −246 −325 −407 −456 −510

Uncracked sections 127 4.4.4 Example application (AEMM) – Approach 2 As discussed for the SSM, approach 2 involves expressing the constitutive relationship in terms of the initial stress σc (τ0 ) and ﬁnal stress σc (t). Eq. 4.36a is re-expressed as: ε(t) = =

σc (t) − σc (τ0 ) σc (τ0 ) + + εsh (t) Ee (t, τ0 ) Ee (t, τ0 ) σc (τ0 )ϕ(t, τ0 )[1 − χ(t, τ0 )] σc (t)[1 + χ (t, τ0 )ϕ(t, τ0 )] + + εsh (t) Ec (τ0 ) Ec (τ0 )

(4.44)

and rearranging gives: Ee (t, τ0 )[ε(t) − εsh (t)] + σc (τ0 ) Fe,0 σc (t) =

(4.45)

where Fe,0 = ϕ(t, τ0 )

[χ(t, τ0 ) − 1] [1 + χ (t, τ0 )ϕ(t, τ0 )]

(4.46)

The steel stress is given by Eq. 4.37b: σs (t) = Es εs (t) and, from Eqs 4.4 and 4.5, the equilibrium and compatibility requirements at time t are: P = σc (t)Ac + σs (t)As and εs (t) = ε(t) Solving for ε(t) gives: 1 ε(t) = 1 + n¯ e,0 ρ

σc (τ0 ) Fe,0 n¯ e,0 − + εsh (t) Es Ac Ee (t, τ0 ) P

(4.47)

By substituting Eqs 4.45, 4.37b and 4.5 into Eq. 4.4, the concrete stress at time t can be expressed as: σc (t) =

1 1 + n¯ e,0 ρ

P + σc (τ0 ) Fe,0 n¯ e,0 ρ − εsh (t) Es ρ Ac

(4.48)

where ρ = As /Ac , and n¯ e,0 = Es /Ee (t, τ0 ) = the age-adjusted modular ratio. The steel stress σs (t) is determined by substituting εs (t) = ε(t) into Eq. 4.37b or by enforcing the requirements of equilibrium (Eq. 4.4).

128 Uncracked sections

Example 4.5 Example 4.4 is repeated here using the AEMM approach 2. As before: Ec (τ0 ) = Ee (τ0 ) = 26.7 GPa; σc (τ0 ) = −9.67 MPa; σs (τ0 ) = −72.3 MPa; εs (τ0 ) = −361 × 10−6 and ε(τ0 ) = −361 × 10−6 .

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53, χ (t, τ0 ) = 0.60 and εsh (t) = −142 × 10−6 . Ee (t, τ0 ) = Ec (τ0 )/(1 + χ (t, τ0 )ϕ(t, τ0 )) = 20.27 GPa; and n¯ e,0 = Es / Ee (t, τ0 ) = 9.87. [0.60 − 1] From Eq. 4.46: Fe,0 = 0.53 = −0.160 [1 + 0.60 × 0.53)] Eq. 4.48 gives: 1 −1000 × 103 σc (t) = − 9.67 × (−0.160) × 9.87 × 0.02 1 + 9.87 × 0.02 90,000 + 142 × 10−6 × 200,000 × 0.02 = −8.55 MPa Eq. 4.4: Eq. 4.36b: Eq. 4.5:

σs (t) = (−1000 × 103 + 8.55 × 90,000)/1800 = −128.0 MPa; εs (t) = −128.0/200,000 = −640 × 10−6 ; and ε(t) = −640 × 10−6 .

The results of the analysis are identical to those obtained using approach 1.

4.5 The rate of creep method (RCM) 4.5.1 Formulation The rate of creep method was originally proposed by Glanville (Ref. 10) and further developed by Whitney (Ref. 11) in the early 1930s to describe the time-varying behaviour of concrete. Dischinger (Ref. 12) ﬁrst applied the method to the analysis of concrete structures. The RCM is based on the assumption that the rate of change of creep with time, dϕ(t, τ0 )/dt(≡ ϕ(t, ˙ τ )), is independent of the age at loading, τ . This means that creep curves for concrete loaded at different times are assumed to be parallel, as shown in Fig 4.10. This, of course, is not true. Better agreement with actual behaviour is obtained by assuming that creep curves for concrete loaded at different times are afﬁne rather than parallel, that is, they are assumed to have the same shape. However, by assuming that the rate of creep is independent of the age at loading, only a single creep curve is required to calculate creep strains due to any stress history.

Uncracked sections 129 j (t,t0)

j (t,t)

F

j (t,t0)

E

B Actual

D

A t0

j (t,ti) (assumed)

ti

j (t,ti) = j (t,t0)

C t

Time

Figure 4.10 Parallel creep curves assumed in the rate of creep method.

Consider the parallel creep curves of Fig. 4.10. Since the ordinates EF and CD are assumed to be equal, CD = CF – AB or: ϕ(t, τi ) = ϕ (t, τ0 ) − ϕ (τi , τ0 )

(4.49)

The creep–time curve caused by a stress applied at any age τi is thus completely deﬁned by a single curve ϕ(t, τ0 ), where τ0 is usually taken to be the age at ﬁrst loading. The creep strain at time t caused by a constant stress σc (τi ) applied at τi is therefore taken to be: εcr (t, τi ) =

σc (τi ) σc (τi ) ϕ(t, τi ) = [ϕ (t, τ0 ) − ϕ (τi , τ0 )] Ec (τ0 ) Ec (τ0 )

(4.50)

and the change in creep strain between any two time instants t1 and t2 after the loading at τi is: εcr (t, τi ) = εcr (t2 , τi ) − εcr (t1 , τi ) =

σc (τi ) [ϕ (t2 , τ0 ) − ϕ (t1 , τ0 ) ] Ec (τ0 )

(4.51)

If a continuously varying stress history is divided into small time intervals δt and the stress during each interval is considered to be constant, the change of creep strain during any time interval is given by Eq. 4.51. In the limit, as δt approaches zero, the rate of change of creep depends only on the current stress and the rate of change of the creep coefﬁcient and is given by: d εcr (t, τ ) σc (t) d ϕ (t, τ0 ) σc (t) = or ε˙ cr (t, τ ) = ϕ(t, ˙ τ0 ) dt Ec (τ0 ) dt Ec (τ0 )

(4.52)

The rate of change of the instantaneous strain at any time depends on the rate of change of stress: d εe (t) σ˙ c (t) 1 d σc (t) = or ε˙ e (t) = dt Ec (τ0 ) d t Ec (τ0 ) where the elastic modulus of concrete is here assumed to be constant in time.

(4.53)

130 Uncracked sections If it is further assumed that shrinkage develops at the same rate as creep (i.e. the creep and shrinkage curves are afﬁne), then: εsh (t) =

εsh (∞) ϕ (t, τ0 ) ϕ(∞, τ0 )

(4.54)

and the time rate of change of shrinkage is given by: ε˙ sh (t) =

ε∗ εsh (∞) ϕ˙ (t, τ0 ) = ∗ sh ϕ˙ (t, τ0 ) ϕ(∞, τ0 ) φ (τ0 )

(4.55)

The rate of change of the total concrete strain may be expressed as the sum of the rates of change of each of the three strain components given by Eqs 4.52, 4.53 and 4.55:

ε∗ σ˙ c (t) σc (t) ε˙ (t, τ ) = + ϕ(t, ˙ τ0 ) + ∗ sh (4.56) Ec (τ0 ) Ec (τ0 ) ϕ (τ0 ) This ﬁrst order differential equation is a constitutive relationship for concrete that can be readily included in structural analysis. The solution of the resulting differential equations is easily obtained for a variety of practical problems. Eq. 4.56 may be rewritten with the creep coefﬁcient ϕ (≡ ϕ (t, τ )) as the independent variable: ε∗ d ε (t, τ ) 1 d σc (t) σc (t) = + + ∗ sh dϕ Ec (τ0 ) d ϕ Ec (τ0 ) ϕ (τ0 )

(4.57)

Eqs 4.56 and 4.57 were developed by Dischinger (Ref. 12) and this type of differential constitutive relationship for concrete is often referred to as Dischinger’s equation of state. 4.5.2 Discussion The rate of creep method, although mathematically attractive, has several deﬁciencies. The assumption of parallel creep curves causes a signiﬁcant underestimation of creep in old concrete. As time increases, ϕ˙ (t, τ0 ) approaches zero and, according to the RCM, so too does the creep strain for concrete loaded at times much later than τ0 . This is not so. Old concrete does creep, albeit much less than young concrete. The RCM therefore underestimates creep for an increasing stress history. This error may be large if signiﬁcant increases of stress occur at times τi >> τ0 . Eq. 4.52 also implies that when stress is removed, the rate of change of creep is zero, that is, creep recovery is not predicted. Creep strains are therefore overestimated for a decreasing stress history. However, for the many practical situations in which loads are applied on relatively young concrete and the stress does not vary too much with time, the RCM gives excellent results. 4.5.3 Example application (RCM) The rate of creep analysis of the column shown in Fig. 4.1 follows the same general steps as the elastic analysis described in Section 4.2.2. However, since the constitutive

Uncracked sections 131 relationship for concrete is in differential form (Eq. 4.56), it is convenient to also express the equilibrium and compatibility equations in this form. For clarity, the arguments t and τ0 are omitted from the various functions in the following analysis. Noting that the rate of change of the applied load P with time is zero, differentiating the equilibrium equation with respect to time gives: ˙ c +N ˙ s = σ˙ c Ac + σ˙ s As = 0 P˙ = N

(4.58)

For compatibility, the rates of change of concrete and steel strains are identical, that is: ε˙ = ε˙ s

(4.59)

and the constitutive relationships for both the concrete and the steel are: ε˙ =

σ˙ c + ϕ˙ Ec

∗ σc εsh + ∗ Ec ϕ

and ε˙ s =

σ˙ s Es

(4.60)

∗ = ε (∞); and ϕ ∗ = ϕ (∞, τ ). From Eq. 4.58: where ϕ˙ = ϕ˙ (t, τ0 ) ; εsh 0 sh

σ˙ s = − σ˙ c

Ac σ˙ c =− As ρ

(4.61)

and substituting Eqs 4.60 and 4.61 into Eq. 4.59 gives: −

∗ σ˙ c σc εsh σ˙ c + ϕ˙ + ∗ = Es ρ E c Ec ϕ

Multiplying by Ec and gathering like terms yields: σ˙ c −nρ = ϕ˙ σc + S 1 + nρ

(4.62)

where: S=

∗ E εsh c

(4.63)

ϕ∗

Integrating both sides of Eq. 4.62 with respect to time gives: nρ ln(σc + S) tt=τ0 = − ϕ tt=τ0 1 + nρ Solving for concrete stress gives: −nρ σc (t) + S = e 1+nρ σc (τ0 ) + S

ϕ (t,τ0 )

i.e. ln

σc (t) + S nρ =− ϕ (t, τ0 ). σc (τ0 ) + S 1 + nρ

132 Uncracked sections and therefore: −nρ

σc (t) = (σc (τ0 ) + S) e 1+nρ

ϕ(t,τ0 )

−S

(4.64)

With the concrete stress obtained from Eq. 4.64, the steel stress may be found from Eq. 4.4 and the steel strain from Eq. 4.6b. Compatibility requires that the concrete strain is the same as the steel strain.

Example 4.6 The symmetrically reinforced column subjected to a constant sustained axial load P that was analysed in Example 4.1 (see Fig. 4.1) is to be re-analysed using the RCM. As before: P = −1000 kN, Ac = 90,000 mm2 ; As = 1800 mm2 ; ρ = As /Ac = 0.02; Ec (τ0 ) = 26.7 GPa; Es = 200 GPa; n = Es /Ec (τ0 ) = 7.48; and ∗ = −510 × 10−6 . εsh The variations of the creep coefﬁcient with time is: (t − τ0 ) in days

0

10

30

70

200

500

10,000 (∞)

ϕ(t, τ0 )

0

0.53

0.98

1.38

1.83

2.10

2.39

The constants in Eq. 4.64 are: and from Eq. 4.62: S =

nρ 7.48 × 0.02 = = 0.130; 1 + nρ 1 + 7.48 × 0.02

−510 × 10−6 × 26,700 = −5.71 MPa. 2.39

At ﬁrst loading, (t − τ0 ) = 0: ϕ(t, τ0 ) = 0; εsh (t) = 0 σc (τ0 ) = −9.67 MPa; σs (τ0 ) = −72.3 MPa; εs (τ0 ) = −361 × 10−6 and ε(τ0 ) = −361 × 10−6 .

At (t − τ0 ) = 10 days: ϕ(t, τ0 ) = 0.53 Eq. 4.64: Eq. 4.4: Eq. 4.6b: Eq. 4.5:

σc (t) = (−9.67 − 5.71)e−0.130×0.53 + 5.71 = −8.65 MPa; −1000 × 10−3 + 8.65 × 90,000 = 123.3 MPa; 1800 −123.3 εs (t) = = −616 × 10−6 ; 200,000

σs (t) =

ε(t) = −616 × 10−6 .

Uncracked sections 133 The elastic and shrinkage components of the total concrete strain are εe (t) = σc (t)/Ec (τ0 ) = −323 × 10−6 ; from Eq. 4.54, the shrinkage component of strain is εsh (t) = (0.53/2.39) × (−510 × 10−6 ) = −113 × 10−6 (since the creep and shrinkage curves are assumed to be afﬁne); and therefore the creep component of strain is εcr (t) = ε(t) − εe (t) − εsh (t) = −180 × 10−6 . It is noted that in this example using RCM, because of the assumption that the creep and shrinkage curves have the same shape, different levels of shrinkage from those speciﬁed in the previous examples occur during each time step. The results of the analyses at ﬁrst loading and throughout the period of sustained loading are as follows: Time t (days)

Duration of load t − τ0 (days)

Concrete stress σc (t) (MPa)

Steel stress σs (t) (MPa)

14 24 44 84 214 514 10,014

0 10 30 70 200 500 10,000

−9.67 −8.65 −7.83 −7.14 −6.41 −5.99 −5.56

−72.3 −123 −164 −198 −235 −256 −278

Total Elastic strain concrete ε(t) strain εe (t) (×10−6 ) (×10−6 ) −361 −616 −820 −992 −1175 −1279 −1388

−361 −323 −293 −267 −240 −224 −208

Creep Shrinkage strain strain εcr (t) εsh (t) (×10−6 ) (×10−6 ) 0 −180 −319 −431 −544 −607 −670

0 −113 −209 −294 −391 −448 −510

4.6 Comparison of methods of analysis A comparison of the numerical results calculated using each method of analysis for the axially loaded column section considered in Examples 4.1–4.6 is provided in Table 4.1. The prediction of time-dependent redistribution of stresses and the gradual development of creep strain with time are compared in Figs 4.11 and 4.12, respectively. A large redistribution of stresses is predicted by all of the methods of analysis. In this axially loaded column, the concrete stress decreases substantially with time and the steel stress increases dramatically. At initial loading, the concrete in the section carried 87 per cent of the total load. After 10,000 days under load, this has reduced to 59.3 per cent (according to the AEMM, for example). During this same time period, the steel stress increased from 72.3 MPa to 269 MPa. This is, in fact, typical of the redistribution of stresses that takes place with time in reinforced concrete structures. The concrete and steel stresses obtained using the AEMM at any time t are almost identical with those predicted by the much more laborious SSM (calculated with 18 intervals). This is not surprising; since the ageing coefﬁcients were determined from the concrete stress changes calculated using the SSM. However, if one assumes that the ageing coefﬁcient is constant and equal to 0.65 at every value of t, as suggested by Eq. 4.43, the AEMM predicts stresses and total strains to within 1 per cent of these more reﬁned values.

134 Uncracked sections Table 4.1 Comparisons of calculated stresses and strains (Examples 4.1–4.6) Method of analysis

Duration of load (days)

Concrete stress σc (τi ) (MPa)

Steel stress σs (τi ) (MPa)

Total strain ε(τi ) (×10−6 )

Elastic strain εe (τi ) (×10−6 )

Creep strain εcr (τi ) (×10−6 )

Shrinkage strain εsh (τi ) (×10−6 )

Effective modulus method (EMM)

0 10 30 70 200 500 10,000

−9.67 −8.58 −7.82 −7.23 −6.66 −6.35 −6.02

−72.3 −127 −165 −194 −222 −238 −255

−361 −633 −824 −969 −1112 −1191 −1273

−361 −321 −292 −270 −249 −237 −225

0 −170 −285 −374 −456 −497 −538

0 −142 −246 −325 −407 −456 −510

Ageadjusted effective modulus method (AEMM)

0 10 30 70 200 500 10,000

−9.67 −8.55 −7.74 −7.10 −6.48 −6.12 −5.73

−72.3 −128 −169 −200 −232 −249 −269

−361 −640 −843 −1002 −1158 −1247 −1346

−361 −320 −289 −266 −242 −229 −214

0 −178 −308 −411 −509 −563 −622

0 −142 −246 −325 −407 −456 −510

0 10 30 70 200 500 10,000

−9.67 −8.55 −7.72 −7.09 −6.46 −6.10 −5.71

−72.3 −128 −169 −201 −233 −251 −270

−361 −641 −847 −1006 −1164 −1253 −1349

−361 −320 −292 −270 −249 −238 −226

0 −179 −309 −411 −508 −559 −613

0 −142 −246 −325 −407 −456 −510

0 10 30 70 200 500 10,000

−9.67 −8.65 −7.83 −7.14 −6.41 −5.99 −5.56

−72.3 −123 −164 −198 −235 −256 −278

−361 −616 −820 −992 −1175 −1279 −1388

−361 −323 −293 −267 −240 −224 −208

0 −180 −319 −431 −544 −607 −670

0 −113 −209 −294 −391 −448 −510

Step-by-step method (SSM)

Rate of creep method (RCM)

Figure 4.12 conﬁrms that the EMM underestimates creep strains for a decreasing stress history, predicting full creep recovery as the stress reduces. The EMM predicts the smallest creep strain at any time t > τ and the smallest eventual stress redistribution (see Fig. 4.11). By contrast, the RCM overestimates creep for this decreasing stress history because it does not allow for any creep recovery. The RCM predicts the largest creep strain and the largest stress redistribution. However, for this simple example, good results are obtained using the RCM at all times after loading with relatively little computational effort. It is noted that the magnitudes of the stresses and deformations predicted by the SSM and the AEMM lie between the magnitudes predicted by the EMM (which is known to underestimate the effects of creep for a decreasing stress history) and the magnitudes predicted by the RCM (which is known to overestimate the effects of creep). Although the total strain predicted by the AEMM and the SSM are almost identical, the elastic strain is different. The AEMM assumes that the total change of stress is applied at τ0 and so the elastic strain at any time t is taken as the concrete stress at that time divided

Uncracked sections 135

Concrete stress (MPa)

−10 EMM AEMM SSM RCM

−8

−6

−4 200

0

400 600 Duration of load (t − t) (days)

1000

Steel stress (MPa)

−300

−200 EMM AEMM SSM RCM

−100

0 0

200

400 600 Duration of load (t − t) (days)

1000

Figure 4.11 Stress redistributions in axially loaded column examples.

Creep strain (×10−6)

−750

−500 EMM AEMM SSM RCM

−250

0 0

200

400

600

1000

Duration of load (t − t) (days)

Figure 4.12 Creep strain versus time in the axially loaded column examples.

136 Uncracked sections by the elastic modulus at τ0 . In the SSM, the elastic strain caused by a change of stress at any time t(> τ0 ) is calculated using the elastic modulus at that time. Therefore, in the example considered here, with a decreasing stress history, the AEMM slightly underestimates the elastic strain predicted by the SSM and, as a consequence, slightly overestimates the creep strain. The results from the SSM depend on the number of time steps considered and the shape of the numerous creep coefﬁcient versus time curves required for the analysis. More accurate results are obtained as the number of time steps increases. The increased amount of input data required and the considerable extra computational effort associated with the SSM normally make it suitable only for computer applications. For manual calculations, the AEMM has much to recommend it. It is usually the most satisfactory alternative in terms of both efﬁciency and accuracy and can be easily incorporated into most existing structural analysis packages.

4.7 References 1. Faber, O. (1927). Plastic yield, shrinkage and other problems of concrete and their effects on design. Minutes of the Proceedings of the Institution of Civil Engineers, 225, Part I, London, 27–23. 2. Ghali, A., Neville, A.M. and Jha, P.C. (1967). Effect of elastic and creep recoveries of concrete on loss of prestress. ACI Journal, 64, 802–810. 3. Comité Euro-International du Béton (1984). CEB Design Manual on Structural Effects of Time-Dependent Behaviour of Concrete. Georgi Publishing, Saint-Saphorin, Switzerland. 4. Ghali, A., Favre, R. and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London. 5. Kawano, A. and Warner, R.F. (1996). Model formulations for numerical creep calculations for concrete. Journal of Structural Engineering, 122(3), 284–290. 6. Trost, H. (1967). Auswirkungen des Superpositionsprinzips auf Kriech- und RelaxationsProbleme bei Beton und Spannbeton. Beton- und Stahlbetonbau, 62(10), 230–238, No. 11, 261–269. 7. Dilger, W. and Neville, A.M. (1971). Method of creep analysis of structural members. ACI SP 27-17, 349–379. 8. Bazant, Z.P. (1972). Prediction of concrete creep effects using age-adjusted effective modulus method. ACI Journal, 69, April, 212–217. 9. Neville, A.M., Dilger, W.H. and Brooks, J.J. (1983). Creep of Plain and Structural Concrete. Construction Press (Longman Group Ltd), London. 10. Glanville, W.H. (1930). Studies in Reinforced Concrete – III, The Creep or Flow of Concrete under Load. Building Research Technical Paper No. 12, Department of Scientiﬁc and Industrial Research, London. 11. Whitney, C.S. (1932). Plain and reinforced concrete arches. ACI Journal, 28, 479–519. 12. Dischinger, F. (1937). Untersuchungen über die Knicksicherheit, die elastische Verformung und das Kriechen des Betons bei Bogenbrücken. Der Bauingenieur, 18(33/34), 487–529 and No. 35/36, 539–552 and No.39/40, 595–621.

5

Uncracked sections Axial force and uniaxial bending

5.1 Introductory remarks In this chapter, time analyses are presented for a variety of uncracked cross-sections containing at least one axis of symmetry and subjected to axial load and uniaxial bending. The concrete is assumed to be able to carry any applied tension and is therefore uncracked. Symmetrically reinforced and asymmetrically reinforced sections containing any number of levels of both non-prestressed and prestressed reinforcement are considered. Composite steel–concrete and composite concrete–concrete sections are also examined. The proposed methods of analysis are based on the assumptions of the Euler– Bernoulli beam theory, in which plane sections are assumed to remain plane and perpendicular to the beam axis before, and after, both short- and long-term deformations. This means that the strain distributions on the cross-section, both immediately upon loading and after a prolonged period of sustained loading and shrinkage, are assumed to be linear.

5.2 Overview of cross-sectional analysis Cross-sectional analysis is used extensively for modelling structural response at both service and ultimate load conditions. With this approach, the governing equilibrium equations describing the behaviour of any cross-section are expressed in terms of two unknowns that deﬁne the strain diagram. These unknowns can be identiﬁed by a single value of strain measured at the level of the reference axis εr and the slope of the strain diagram κ (which is, of course, the curvature of the cross-section). Considering the cross-section shown in Fig. 5.1a, the section is symmetrical about the y-axis and the orthogonal x-axis is selected as the reference axis. If the cross-section is subjected to an axial force applied at the origin of the x- and y-axes and a bending moment applied about the x-axis, the strain diagram is shown in Fig. 5.1b and the strain at any depth y below the reference axis is given by: ε = εr + yκ

(5.1)

The two unknowns of the problem, εr and κ, are then determined by enforcing horizontal and rotational equilibrium at the cross-section: Ni = Ne

(5.2a)

138 Uncracked sections er e

x Area, A y (a) Cross-section

k

y (b) Strain diagram

Figure 5.1 Generic cross-section.

and Mi = Me

(5.2b)

where Ne and Me denote the external axial force and moment, respectively, at the section and Ni and Mi are the internal axial force and moment, respectively, given by: Ni =

A

σ dA

(5.3a)

yσ dA

(5.3b)

and Mi =

A

When the two unknowns (εr and κ) are calculated from the two equilibrium equations (Eqs 5.2) and the strain is determined using Eq. 5.1, the stresses in the concrete and steel may be obtained from the appropriate constitutive relationships. The internal actions are then readily determined from the stresses using Eqs 5.3. This procedure forms the basis of both the short- and long-term analyses presented in the remainder of this chapter.

5.3 Short-term analysis of reinforced or prestressed concrete cross-sections The short-term analysis of an uncracked reinforced or prestressed concrete crosssection at service loads is usually made assuming linear-elastic behaviour of the concrete (in compression and tension) and linear-elastic behaviour of the nonprestressed reinforcement and the prestressing steel. The procedure can be applied to typical cross-sections such as those shown in Fig. 5.2. Without any loss of generality, it is assumed that the contribution of each reinforcing bar or prestressing tendon is lumped into layers according to its location, as shown in Fig. 5.3. The numbers of layers of non-prestressed and prestressed reinforcement are ms and mp , respectively. In Fig. 5.3b, ms = 3 and mp = 2. In particular, the properties of each layer of non-prestressed reinforcement are deﬁned by its area, elastic modulus and location with respect to the arbitrarily chosen x-axis and are labelled as As(i) , Es(i) and

Uncracked sections 139

Typical prestressed steel reinforcement

Typical non-prestressed steel reinforcement

Figure 5.2 Typical reinforced and prestressed concrete sections.

ys(i) , respectively. With this notation the subscript ‘s’ stands for (non-prestressed) steel reinforcement and i = 1, . . . , ms . Similarly, Ap(i) , Ep(i) and yp(i) represent, respectively, the area, elastic modulus and location of the prestressing steel with respect to the x-axis and i = 1, . . . , mp . The geometric properties of the concrete part of the cross-section are Ac , Bc and Ic , which denote the area and the ﬁrst and second moments of area of the concrete about the x-axis, respectively. For the short-term or instantaneous analysis, assumed to take place at time τ0 , the linear-elastic stress-strain relationships of the concrete and the steel are: σc,0 = Ec,0 ε0

(5.4a)

σs(i),0 = Es(i) ε0 σp(i),0 = Ep(i) ε0 + εp(i),init

(5.4b) (5.4c)

in which σc,0 , σs(i),0 and σp(i),0 represent the stresses in the concrete, in the i-th layer of non-prestressed reinforcement (with i = 1, . . . , ms ) and in the i-th layer of prestressing steel (with i = 1, . . . , mp ), respectively, immediately after ﬁrst loading at time τ0 , while

Non-prestressed steel reinforcement ds(1) ys(1) ys(2)

ds(2) Concrete

As(1) As(2)

Ac, Bc, Ic dp(1) dp(2) ds(3)

x

Prestressed steel reinforcement Non-prestressed steel reinforcement

yp(1) yp(2)

Ap(1) Ap(2) As(3)

ys(3)

y (a) Generic cross-section

(b) The contribution of each reinforcement bar or tendon is lumped into layers located ys(i) and yp(i) from the reference axis (x-axis)

Figure 5.3 Generic cross-section and arrangement of reinforcement.

140 Uncracked sections εp(i),init is the initial strain in the i-th layer of prestressing steel produced by the initial tensile prestressing force Pp(i),init (i.e. the prestressing force before the prestress is transferred to the concrete) and given by: εp(i),init =

Pp(i),init Ap(i) Ep(i)

(5.5)

With this method, the prestressing force is included in the analysis by means of an induced strain εp(i),init rather than as an external action (Refs 1 and 2). For the short-term analysis at time τ0 , the internal axial force and moment resisted by the cross-section about the reference axis are denoted Ni,0 and Mi,0 , respectively. The internal axial force Ni,0 is the sum of the axial forces resisted by the component materials forming the cross-section and is given by: Ni,0 = Nc,0 + Ns,0 + Np,0

(5.6)

where Nc,0 , Ns,0 and Np,0 represent the axial forces resisted by the concrete, the nonprestressed reinforcement and the prestressing steel, respectively, and are calculated from: Nc,0 = Ns,0 =

Ac

σc,0 dA =

Ac

Ec,0 (εr,0 + yκ0 ) dA = Ac Ec,0 εr,0 + Bc Ec,0 κ0

(5.7a)

ms ms ms As(i) Es(i) εr,0 + ys(i) κ0 = As(i) Es(i) εr,0 + ys(i) As(i) Es(i) κ0 i=1

i=1

i=1

(5.7b) mp mp mp Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(i) Ep(i) εp(i),init Np,0 = i=1

i=1

(5.7c)

i=1

where the additional subscripts ‘0’ used for the strain at the level of the reference axis (εr,0 ) and the curvature (κ0 ) highlight that these are calculated at time τ0 after the application of Ne,0 and Me,0 and after the transfer of prestress. By substituting Eqs 5.7 into Eq. 5.6, the equation for Ni,0 is expressed in terms of the actual geometry and elastic moduli of the materials forming the cross-section: Ni,0 = Ac Ec,0 +

ms

As(i) Es(i) +

i=1

+ Bc Ec,0 +

ms

mp

Ap(i) Ep(i) εr,0

i=1

ys(i) As(i) Es(i) +

mp

yp(i) Ap(i) Ep(i) κ0 +

i=1

i=1

mp Ap(i) Ep(i) εp(i),init i=1

mp

= RA,0 εr,0 + RB,0 κ0 +

Ap(i) Ep(i) εp(i),init i=1

(5.8)

Uncracked sections 141 in which RA,0 and RB,0 represent, respectively, the axial rigidity and the stiffness related to the ﬁrst moment of area about the reference axis calculated at time τ0 and are given by: RA,0 = Ac Ec,0 +

ms

As(i) Es(i) +

mp

i=1

RB,0 = Bc Ec,0 +

ms

Ap(i) Ep(i)

(5.9a)

i=1

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

(5.9b)

i=1

Similarly, the equation for Mi,0 may be expressed as: mp ms Mi,0 = Bc Ec,0 + ys(i) As(i) Es(i) + yp(i) Ap(i) Ep(i) εr,0

i=1

+ Ic Ec,0 +

ms

i=1 mp 2 ys(i) As(i) Es(i) +

i=1

+

2 yp(i) Ap(i) Ep(i)

κ0

i=1

mp yp(i) Ap(i) Ep(i) εp(i),init i=1

= RB,0 εr,0 + RI,0

mp yp(i) Ap(i) Ep(i) εp(i),init κ0 +

(5.10)

i=1

where RI,0 is the ﬂexural rigidity at time τ0 given by: RI,0 = Ic Ec,0 +

ms i=1

2 ys(i) As(i) Es(i) +

mp

2 yp(i) Ap(i) Ep(i)

(5.11)

i=1

Substituting the expressions for Ni,0 and Mi,0 (Eqs 5.8 and 5.10) into Eqs 5.2 produces the system of equilibrium equations that may be written in compact form as: re,0 = D0 ε0 + fp,init

(5.12)

where

Ne,0 re,0 = Me,0

RA,0 RB,0 D0 = RB,0 RI,0

εr,0 ε0 = κ0 mp Ap(i) Ep(i) εp(i),init fp,init = yp(i) Ap(i) Ep(i) εp(i),init i=1

(5.13a) (5.13b) (5.13c)

(5.13d)

142 Uncracked sections The vector re,0 is the vector of the external actions at ﬁrst loading (at time τ0 ), i.e. axial force Ne,0 and moment Me,0 ; the matrix D0 contains the cross-sectional material and geometric properties calculated at τ0 ; the strain vector ε0 contains the unknown independent variables describing the strain diagram at time τ0 (εr,0 and κ0 ); and the vector f p,init contains the actions caused by the initial prestressing. The vector ε0 is readily obtained by solving the equilibrium equations (Eq. 5.12) giving: re,0 − fp,init = F0 re,0 − fp,init (5.14) ε0 = D−1 0 where F0 =

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

−RB,0 RA,0

(5.15)

The stress distribution related to the concrete and reinforcement can then be calculated from the constitutive equations (Eqs 5.4) re-expressed here as: σc,0 = Ec,0 ε0 = Ec,0 [1

y]ε0

σs(i),0 = Es(i) ε0 = Es(i) [1 ys(i) ]ε0 σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) [1

(5.16a) (5.16b) yp(i) ] ε0 + Ep(i) εp(i),init

(5.16c)

where ε0 = εr,0 + yκ0 = [1 y] ε0 . Although this procedure is presented here assuming linear-elastic material properties, it is quite general and is also applicable to non-linear material behaviour, in which case the integrals of Eqs 5.3 might have to be evaluated numerically. However, when calculating the short-term response of uncracked reinforced and prestressed concrete cross-sections under typical in-service loads, material behaviour is essentially linear elastic. In reinforced and prestressed concrete design, it is common to calculate the crosssectional properties by transforming the section into equivalent areas of one of the constituent materials. For example, for the cross-section of Fig. 5.3a, the transformed concrete cross-section for the short-term analysis is shown in Fig. 5.4, with the area of each layer of bonded steel reinforcement and tendons (As(i) and Ap(i) , respectively) transformed into equivalent areas of concrete (ns(i),0 As(i) and np(i),0 Ap(i) , respectively), where ns(i),0 = Es(i) /Ec,0 is the modular ratio of the i-th layer of non-prestressed steel and np(i),0 = Ep(i) /Ec,0 is the modular ratio of the i-th layer of prestressing steel. For the transformed section of Fig. 5.4, the cross-sectional rigidities deﬁned in Eqs 5.9 and 5.11 can be re-calculated as: RA,0 = A0 Ec,0

(5.17a)

RB,0 = B0 Ec,0

(5.17b)

RI,0 = I0 Ec,0

(5.17c)

where A0 is the area of the transformed concrete section, and B0 and I0 are the ﬁrst and second moments of the transformed area about the reference x-axis at ﬁrst loading.

Uncracked sections 143 (ns(1),0 −1)As(1) (ns(2),0 −1)As(2)

x (np(1),0 −1)A(1) (np(2),0 −1)Ap(2)

if bonded

(ns(3),0 −1)As(3)

y

Figure 5.4 Transformed section with bonded reinforcement transformed into equivalent areas of concrete.

Substituting Eqs 5.17 into Eq. 5.15 enables F0 to be expressed in terms of the properties of the transformed concrete section as:

I0 F0 = 2 Ec,0 (A0 I0 − B0 ) −B0 1

−B0 A0

(5.18)

The two approaches proposed for the calculation of the cross-sectional rigidities, i.e. the one based on Eqs 5.9 and 5.11 and the one relying on the properties of the transformed section (Eqs 5.17), are equivalent. The procedure based on the transformed section (Eqs 5.17) is often preferred for the analysis of reinforced and prestressed concrete sections, while for composite steel–concrete and concrete–concrete cross-sections, the procedure based on Eqs 5.9 and 5.11 is generally more convenient. The use of both approaches is illustrated in the following examples.

Example 5.1 For the reinforced concrete section shown in Fig. 5.5, the strain and stress distributions are to be determined immediately after application of an axial force Ne,0 = −30 kN and a sagging (positive) bending moment of Me,0 = 50 kNm, applied with respect to the x-axis located 200 mm below the top ﬁbre of the cross-section. Both the concrete and reinforcement are assumed to be linearelastic with Ec,0 = 25 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = ns(1),0 = ns(2),0 = Es /Ec,0 = 8. For this reinforced concrete cross-section, f p,init is a nil vector and the vector of external actions is: −30 × 103 N re,0 = 50 × 106 Nmm

144 Uncracked sections b = 300 ds(1) = 50 As(1) = 620 mm2 dref = 200 x D = 600

ys(1) = −150 ys(2) = +350

ds(2) = 550

As(2) = 1800 mm2

y

Figure 5.5 Reinforced concrete cross-section for Example 5.1 (dimensions in mm).

With the steel reinforcement transformed into equivalent areas of concrete, the relevant properties of the transformed cross-section for inclusion in the F0 matrix (Eq. 5.18) are calculated as follows: A0 = bD + (ns,0 − 1)[As(1) + As(2) ] = 300 × 600 + (8 − 1) × [620 + 1800] = 196,900 mm2

D B0 = bD − dref + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] 2 = 300 × 600 × (300 − 200) + (8 − 1) × [620 × (−150) + 1800 × 350] = 21,760 × 103 mm3

2 bD3 D 2 2 I0 = + bD − dref + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] 12 2 =

300 × 6003 + 300 × 600 (300 − 200)2 + (8 − 1) 12 × [620 × (−150)2 + 1800 × 3502 ] = 8841 × 106 mm4

From Eq. 5.18: F0 =

1 25,000 × (196,900 × 8841 × 106 − (21,760 × 103 )2 ) −21,760 × 103 8841 × 106 × 196,900 −21,760 × 103

278.9 × 10−12 N−1 −686.5 × 10−15 N−1 mm−1 = −1 −686.5 × 10−15 N mm−1 6.214 × 10−15 N−1 mm−2

Uncracked sections 145 The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.14:

! −30 × 103 0 278.9 × 10−12 −686.5 × 10−15 ε0 = × − 0 −686.5 × 10−15 6.214 × 10−15 50 × 106

−42.7 × 10−6 = 0.331 × 10−6 mm−1

The strain at the reference axis and the curvature are therefore: εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 and, from Eq. 5.1, the top (y = −200 mm) and bottom (y = +400 mm) ﬁbre strains are: ε0(top) = εr,0 − 200 × κ0 = (−42.7 − 200 × 0.331) × 10−6 = −108.9 × 10−6 ; and ε0(btm) = εr,0 + 400 × κ0 = (−42.7 + 400 × 0.331) × 10−6 = +89.8 × 10−6 . The top and bottom ﬁbre stresses in the concrete and the stresses in the two layers of reinforcement are obtained from Eqs 5.16:

σc,0(top) = Ec,0 1 yc(top)

= −2.72 MPa

σc,0(btm) = Ec,0 1 yc(btm) = 2.25 MPa

σs(1),0 = Es(1) 1 ys(1)

σs(2),0 = Es(2) 1 ys(2) = 14.6 MPa

−42.7 × 10−6 ε0 = 25 × 10 × 1 400 0.331 × 10−6

3

−42.7 × 10−6 ε0 = 200 × 10 × 1 −150 0.331 × 10−6

−42.7 × 10−6 ε0 = 200 × 10 1 350 0.331 × 10−6

= −18.5 MPa

−42.7 × 10−6 ε0 = 25 × 10 × 1 −200 0.331 × 10−6

3

3

3

146 Uncracked sections The results are plotted in Fig. 5.6.

er,0 = −42.7 × 10−6

− 2.72 −18.5 e

x

s

k0 = 0.331 × 10−6 mm−1

14.6 y

y

(a) Cross-section

y

(b) Strain diagram

2.25

(c) Stress diagram (MPa)

Figure 5.6 Strain and stress diagrams for Example 5.1.

The cross-sectional rigidities could have also been calculated using Eqs 5.9 and 5.11 without transforming the section as follows:

RA,0 = Agross Ec,0 +

ms

As(i) (Es(i) −Ec,0 ) = bDEc,0 + As(1) + As(2) (Es − Ec,0 )

i=1

= 300 × 600 × 25,000 + (620 + 1800) × (200,000 − 25,000) = 4923 × 106 N RB,0 = Agross

ms D − dref Ec,0 + ys(i) As(i) (Es(i) − Ec,0 ) 2 i=1

= 300 × 600 ×

600 − 200 × 25,000 + [620 × (−150) + 1800 × 350] 2

× (200,000 − 25,000) = 543.9 × 109 Nmm RI,0 = Igross + Agross

D − dref 2

2 Ec,0 +

ms

2 ys(i) As(i) (Es(i) − Ec,0 )

i=1

300 × 6003 2 = + 300 × 600 (300 − 200) × 25,000 + 620 × (−150)2 12 +1800 × 3502 × (200,000 − 25,000) = 221.0 × 1012 Nmm2

Uncracked sections 147 and F0 can then be obtained from Eq. 5.15 as: F0 = =

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

−RB,0 RA,0

1

2 543.9 × 109 −543.9 × 109 4923 × 106

4923 × 106 × 221.0 × 1012 −

×

221.0 × 1012 −543.9 × 109

278.9 × 10−12 N−1 = −686.5 × 10−15 N−1 mm−1

−686.5 × 10−15 N−1 mm−1 6.214 × 10−15 N−1 mm−2

and this, of course, is identical to that calculated previously using Eq. 5.18.

Example 5.2 The instantaneous stress and strain distributions on the precast pretensioned concrete section shown in Fig. 5.7 are to be calculated. The cross-section is that of a Girder Type 3 from the AS5100.5 (Ref. 3) guidelines, with the area of the gross section Agross = 317 × 103 mm2 and the second moment of area of the gross-section about the centroidal axis Igross = 49,900 × 106 mm4 . The centroid of the gross cross-sectional area is located 602 mm below its top ﬁbre, i.e. dc = 602 mm. The section is subjected to a compressive axial force Ne,0 = −100 kN and a hogging moment of Me,0 = −50 kNm applied with respect to the reference x-axis, that is taken in this example to be 300 mm below the top ﬁbre of the cross-section. All materials are linear-elastic with Ec,0 = 32 GPa and Es = Ep = 200 GPa. The modular ratios of the reinforcing steel and the prestressing steel are therefore ns(i),0 = np(i),0 = 6.25. The prestressing forces applied to the top and bottom tendons (Ap(1) and Ap(2) , respectively) prior to the transfer of prestress are Pp(1),init = Pp(2),init = 1000 kN. The distances of the steel layers from the reference axis are ys(1) = −240 mm, ys(2) = +790 mm, yp(1) = +580 mm and yp(2) = +710 mm. From Eq. 5.5, the initial strains in the prestressing steel layers prior to the transfer of prestress to the concrete are: εp(1),init = εp(2),init =

1000 × 103 = 0.00625 800 × 200 × 103

The vector of external actions at ﬁrst loading is

−100 × 103 N re,0 = −50 × 106 Nmm

148 Uncracked sections As(1) = 900 mm2

ds(1) = 60

dref = 300 dc = 602

x Centroidal axis of precast concrete I-girder

dp(1) = 880

Ap(1) = 800 mm2

dp(2) = 1010 ds(2) = 1090

Ap(2) = 800 mm2 As(2) = 1800 mm2

D = 1150 y

Figure 5.7 Precast prestressed concrete section for Example 5.2 (dimensions in mm).

and, from Eq. 5.13d, the vector of initial prestressing forces is: fp,init =

2 i=1

Ap(i) Ep(i) εp(i),init

yp(i) Ap(i) Ep(i) εp(i),init

800 × 200,000 × 0.00625 800 × 200,000 × 0.00625 + 580 × 800 × 200,000 × 0.00625 710 × 800 × 200,000 × 0.00625 2000 × 103 N = 1290 × 106 Nmm

=

The relevant cross-sectional properties of the transformed section expressed in equivalent concrete areas are: A0 = Agross + (ns,0 − 1)[As(1) + As(2) ] + (np,0 − 1)[Ap(1) + Ap(2) ] = 317 × 103 + (6.25 − 1) × [900 + 1800] + (6.25 − 1) × [800 + 800] = 339.6 × 103 mm2 B0 = Agross (dc − dref ) + (ns,0 − 1)[As(1) ys(1) + As(2) ys(2) ] + (np,0 − 1)[Ap(1) yp(1) + Ap(2) yp(2) ] = 317 × 103 × (602 − 300) + (6.25 − 1) × [900 × (−240) + 1800 × 790] + (6.25 − 1) × [800 × 580 + 800 × 710] = 107.5 × 106 mm3 2 2 I0 = Igross + Agross (dc − dref )2 + (ns,0 − 1)(As(1) ys(1) + As(2) ys(2) ) 2 2 + Ap(2) yp(2) ) = 49,900 × 106 + 317 × 103 + (np,0 − 1)(Ap(1) yp(1)

× (602 − 300)2 + (6.25 − 1) × [900 × (−240)2 + 1800 × 7902 ] + (6.25 − 1) × [800 × 5802 + 800 × 7102 ] = 88,510 × 106 mm4

Uncracked sections 149 From Eq. 5.18: 1 32,000 × (339,600 × 88,510 × 106 − (107.5 × 106 )2 ) 88,510 × 106 −107.5 × 106 × −107.5 × 106 339,600 149.5 × 10−12 N−1 −181.5 × 10−15 N−1 mm−1 = −181.5 × 10−15 N−1 mm−1 573.5 × 10−18 N−1 mm−2

F0 =

The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.14: 149.5 × 10−12 −181.5 × 10−15 ε0 = F0 re,0 − fp,init = −181.5 × 10−15 573.5 × 10−18 ! −100 × 103 2000 × 103 × − −50 × 106 1290 × 106 −70.7 × 10−6 = −0.387 × 10−6 mm−1 The strain at the reference axis and the curvature are therefore εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 and, from Eq. 5.1, the top (y = −300 mm) and bottom (y = +850 mm) ﬁbre strains are: ε0(top) = εr,0 −300×κ0 = (−70.7−300×(−0.387))×10−6 = +45.5×10−6 and ε0(btm) = εr,0 +850×κ0 = (−70.7+850×(−0.387))×10−6 = −399.8×10−6 From Eq. 5.16a, the top and bottom ﬁbre stresses in the concrete are: σc,0(top) = Ec,0 ε0(top) = 32,000 × 45.5 × 10−6 = +1.45 MPa σc,0(btm) = Ec,0 ε0(btm) = 32,000 × (−399.8) × 10−6 = −12.8 MPa and, from Eq. 5.16b, the stresses in the two layers of non-prestressed reinforcement are: −70.7 × 10−6 3 σs(1),0 = 200 × 10 × 1 −240 = 4.5 MPa −0.387 × 10−6 and σs(2),0 = 200 × 10 × 1 790 3

−70.7 × 10−6 = −0.387 × 10−6

−75.3 MPa

150 Uncracked sections The stresses in the two layers of prestressing steel are obtained from Eq. 5.16c: σp(1),0 = Ep 1 yp(1) ε0 + Ep εp(1),init −70.7 × 10−6 3 = 200 × 10 × 1 580 + 200,000 × 0.00625 −0.387 × 10−6 = 1191 MPa and σp(2),0 = Ep 1 yp(2) ε0 + Ep εp(2),init −70.7 × 10−6 3 = 200 × 10 × 1 710 + 200,000 × 0.00625 −0.387 × 10−6 = 1181 MPa. The stress and strain distributions are plotted in Fig. 5.8. +45.5 × 10−6

+1.45 4.5

e

x

s

k0 = −0.387 × 10−6 mm−1

1191 −75.3 −6

−399.8 × 10

y (a) Cross-section

(b) Strain diagram

1181

−12.8 (c) Stress diagram (MPa)

Figure 5.8 Strain and stress diagrams for Example 5.2.

As already outlined in Example 5.1, the cross-sectional rigidities included in F0 can also be calculated based on Eqs 5.9 and 5.11 considering the individual contribution of each component without modifying their geometry (i.e. without transforming the section): RA,0 = Agross Ec,0 + As(1) + As(2) Es − Ec,0 + Ap(1) + Ap(2) Ep − Ec,0 = 10,866 × 106 N RB,0 = Agross dc − dref Ec,0 + As(1) ys(1) + As(2) ys(2) Es − Ec,0 + Ap(1) yp(1) + Ap(2) yp(2) Ep − Ec,0 = 3439 × 109 Nmm 2 2 2 RI,0 = Igross + Agross dc − dref Ec,0 + As(1) ys(1) Es − Ec,0 + As(2) ys(2) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep − Ec,0 = 2832 × 1012 Nmm2

Uncracked sections 151 Matrix F0 can then be determined as (Eq. 5.15): 1

F0 =

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 −181.5 × 10−15 N−1 mm−1 149.5 × 10−12 N−1 = −181.5 × 10−15 N−1 mm−1 573.5 × 10−18 N−1 mm−2

5.4 Long-term analysis of reinforced or prestressed concrete cross-sections using the age-adjusted effective modulus method (AEMM) Cross-sectional analysis using the age-adjusted effective modulus method (see Section 4.4) provides an effective tool for determining how stresses and strains vary with time due to creep and shrinkage of concrete and relaxation of the prestressing steel (if any). For this purpose, two instants in time are identiﬁed, as shown in Fig. 5.9. One time instant is the time at ﬁrst loading, i.e. t = τ0 , and one represents the instant in time at which stresses and strains need to be evaluated, i.e. t = τk . It is usually convenient to measure time in days starting from the time when the concrete is poured. During the time interval tk (= τk − τ0 ), creep and shrinkage strains develop in the concrete and relaxation occurs in the prestressing steel. The gradual change of strain in the concrete with time causes changes of stress in the bonded reinforcement. In general, as the concrete shortens due to compressive creep and shrinkage, the reinforcement is compressed and there is a gradual increase in the compressive stress in the nonprestressed reinforcement and a gradual loss of prestress in any bonded prestressing tendons. To maintain equilibrium, the gradual change of force in the steel at each bonded reinforcement level is opposed by an equal and opposite restraining force on the concrete, as shown in Fig. 5.10. These gradually applied forces (Tc.s(i) and Tc.p(i) ) are usually tensile and, for a prestressed or partially-prestressed cross-section, tend to relieve the concrete of its initial compression. The resultants of the creep and shrinkage-induced internal restraining forces on the concrete are an increment of axial force N(τk ) and an increment of moment about the reference axis M(τk ) given by: N(τk ) =

ms i=1

Tc.s(i) +

mp

Tc.p(i)

(5.19a)

i=1

and M(τk ) =

ms i=1

Tc.s(i) ys(i) +

mp

Tc.p(i) yp(i)

(5.19b)

i=1

Equal and opposite actions −N(τk ) and −M(τk ) are applied to the bonded steel parts of the cross-section.

152 Uncracked sections Duration of load, Dtk =tk−t0 t=0

t0

tk

Concrete pour

First loading

Time instant at which stresses and deformations are sought

Time, t

Figure 5.9 Relevant instants in time (AEMM). erk DTc.s(1)

ys(1)

Der

x ys(2) yp(2)

yp(1)

kk DTc.p(1) DTc.p(2) DTc.s(2)

y Section

Elevation

time, tk

Restraining forces

er0 k0 t0

Strain

Figure 5.10 Time-dependent actions and deformations.

The strain at any depth y below the reference axis at time τk may be expressed in terms of the strain at the reference axis εrk and the curvature κk : εk = εr,k + yκk

(5.20)

The magnitude of the change of strain that occurs with time εk (= εk − ε0 ) is the sum of each of the following components: (a) the free shrinkage strain εsh (τk ) (which is usually considered to be uniform over the section); (b) the unrestrained creep strain caused by the initial concrete stress σc,0 existing at the beginning of the time period, i.e. εcr,k = ϕ(τk , τ0 )σc,0 /Ec,0 ; and (c) the creep and elastic strain caused by N(τk ) and M(τk ) gradually applied to the concrete cross-section throughout the time period. For the time analysis, the steel reinforcement and prestressing tendons (if any) are assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationship for the concrete is that given by Eq. 4.45. The stress-strain relationships for each material at τ0 and at τk are as follows. At τ0 : σc,0 = Ec,0 ε0 σs(i),0 = Es(i) ε0 σp(i) = Ep(i) ε0 + εp(i),init

(5.21a) (5.21b) (5.21c)

Uncracked sections 153 At τk : Fe,0 σc,0 Ee,k εk − εsh,k + σc,k = σs(i),k = Es(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(5.22a) (5.22b) (5.22c)

Ee,k is the age-adjusted effective modulus at t = τk where Fe,0 is given by Eq. 4.46, (Eq. 4.35), and εp.rel(i),k is the tensile creep strain that has developed in the i-th prestressing tendon at time τk (often referred to as the relaxation strain) and may be calculated from: εp.rel(i),k =

Pp(i),init ϕp (τk , σp(i),init ) = εp(i),init ϕp (τk , σp(i),init ) Ap(i) Ep(i)

(5.23a)

where ϕp (τk , σp(i),init ) is the creep coefﬁcient for the prestressing steel at time τk due to an initial stress σp(i),init in the i-th prestressing tendon just prior to transfer (as given in Table 2.7). Alternatively, εp.rel(i),k may be calculated from the relaxation R given in Eq. 2.11 or included in Table 2.7 as: εp.rel(i),k = εp(i),init R

(5.23b)

The governing equations describing the long-term behaviour of a cross-section are obtained by enforcing equilibrium at the cross-section at time τk following the approach already presented in the previous section for the instantaneous analysis at time τ0 (Eqs 5.4–5.18), and by extending the approach outlined for axially loaded uncracked cross-sections in Sections 4.4.1 and 4.4.4. Restating the equilibrium equations (Eqs 5.2) at time τk gives: re,k = ri,k

(5.24)

where

Ne,k Me,k

re,k =

(5.25a)

and

Ni,k ri,k = Mi,k

(5.25b)

Ni,k and Mi,k depict the internal axial force and moment resisted by the cross-section at time τk , while Ne,k and Me,k represent the external applied loads at this time. As in Eq. 5.6, the axial force Ni,k is the sum of the axial forces carried by the concrete, the reinforcement and the tendons: Ni,k = Nc,k + Ns,k + Np,k

(5.26)

154 Uncracked sections Considering the time-dependent constitutive relationship for the concrete (Eq. 5.22a), the axial force resisted by the concrete at time τk can be expressed as: Nc,k = σc,k dA = Ee,k εr,k + yκk − εsh,k + Fe,0 σc,0 d A Ac

Ac

= Ac Ee,k εr,k + Bc Ee,k κk − Ac Ee,k εsh,k + Fe,0 Nc,0

(5.27)

where εr,k and κk are the strain at the level of the reference axis and the curvature at time τk , while Nc,0 is the axial force resisted by the concrete at time τ0 . For the time analysis, Nc,0 is assumed to be known having been determined during the instantaneous analysis from Eq. 5.7a. Using the constitutive equations for the steel (Eqs 5.22b and c), the axial forces carried by the reinforcing bars and the prestressing steel at time τk are calculated as: ms ms Ns,k = As(i) Es(i) εr,k + ys(i) As(i) Es(i) κk i=1

Np,k =

(5.28a)

i=1

mp mp Ap(i) Ep(i) εr,k + yp(i) Ap(i) Ep(i) κk i=1

i=1

mp

+

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.28b)

i=1

By substituting Eqs 5.27 and 5.28 into Eq. 5.26, the internal axial force is given by: mp ms ms As(i) Es(i) + Ap(i) Ep(i) εr,k + Bc Ee,k + ys(i) As(i) Es(i) Ni,k = Ac Ee,k + i=1 mp

+

i=1

i=1

yp(i) Ap(i) Ep(i) κk − Ac Ee,k εsh,k + Fe,0 Nc,0

i=1

+

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

= RA,k εr,k + RB,k κk − Ac Ee,k εsh,k + Fe,0 Nc,0 +

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.29)

i=1

where the axial rigidity and the stiffness related to the ﬁrst moment of area calculated at time τk have been referred to as RA,k and RB,k , respectively, and are given by: Ee,k + RA,k = Ac

ms i=1

RB,k = Bc Ee,k +

ms i=1

As(i) Es(i) +

mp

Ap(i) Ep(i)

(5.30a)

i=1

ys(i) As(i) Es(i) +

mp i=1

yp(i) Ap(i) Ep(i)

(5.30b)

Uncracked sections 155 In a similar manner, the internal moment Mi,k resisted by the cross-section at time τk can be expressed as: mp ms ys(i) As(i) Es(i) + yp(i) Ap(i) Ep(i) εr,k Mi,k = Bc Ee,k + i=1

+ Ic Ee,k +

ms

i=1 2 ys(i) As(i) Es(i) +

i=1

+ Fe,0 Mc,0 +

mp

2 yp(i) Ap(i) Ep(i) κk − Bc Ee,k εsh,k

i=1

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

= RB,k εr,k + RI,k κk − Bc Ee,k εsh,k + Fe,0 Mc,0 +

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(5.31)

i=1

where the ﬂexural rigidity of the cross-section calculated at time τk , referred to as RI,k in Eq. 5.31, is given by: Ee,k + RI,k = Ic

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

(5.32)

i=1

and Mc,0 is the moment resisted by the concrete component at time τ0 and from the instantaneous analysis: yσc,0 dA = yEc,0 εr,0 + yκ0 dA = Bc Ec,0 εr,0 + Ic Ec,0 κ0 (5.33) Mc,0 = Ac

Ac

After substituting Eqs 5.29 and 5.31 into Eq. 5.24, the equilibrium equations at time τk may be written in compact form as: re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k

(5.34)

where

ε εk = r,k κk

and Dk =

RA,k RB,k RB,k RI,k

(5.35a)

(5.35b)

The vector f cr,k represents the creep effect produced by the stress σc,0 resisted by the concrete at time τ0 and is given by:

Nc,0 Ac εr,0 + Bc κ0 = Fe,0 Ec,0 (5.36) Fe,0 fcr,k = Mc,0 Bc εr,0 + Ic κ0

156 Uncracked sections and Fe,0 is given in Eq. 4.46. The vector f sh,k accounts for the uniform shrinkage strain that develops in the concrete over the time period and is given by: fsh,k =

Ac E ε Bc e,k sh,k

(5.37)

The vector f p,init in Eq. 5.34 accounts for the initial prestress and the vector f p.rel,k accounts for the resultant actions caused by the loss of prestress in the tendon due to relaxation. These are given by: fp,init =

mp Ap(i) Ep(i) εp(i),init yp(i) Ap(i) Ep(i) εp(i),init

(5.38a)

i=1

and fp.rel,k = fp,init ϕp (τk , σp(i),init )

(5.38b)

Eq. 5.34 can be solved for εk as: re,k − fcr,k + fsh,k − fp,init + fp.rel,k εk = D−1 k = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(5.39)

where Fk =

1 RA,k RI,k − R2B,k

RI,k −RB,k −RB,k RA,k

The stress distribution at time τk can then be calculated as follows: " # σc,k = Fe,0 σc,0 = Fe,0 σc,0 Ee,k εk − εsh,k + Ee,k 1 y εk − εsh,k + σs,k(i) = Es(i) εk = Es(i) 1 ys(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(5.40)

(5.41a) (5.41b)

(5.41c)

where at any point y from the reference axis εk = εr,k + yκk = 1 y εk . The cross-sectional rigidities RA,k , RB,k and RI,k , required for the solution at time τk can also be calculated from the properties of the age-adjusted transformed section, obtained by transforming the bonded steel areas (reinforcement and tendons) into equivalent areas of the aged concrete at time τk , as follows: Ak Ee,k RA,k =

(5.42a)

RB,k = Bk Ee,k

(5.42b)

RI,k = I¯k Ee,k

(5.42c)

Uncracked sections 157 where Ee,k is the age-adjusted effective modulus, Ak is the area of the age-adjusted transformed section, and Bk and I¯k are the ﬁrst and second moments of the area of the age-adjusted transformed section about the reference axis. For the determination of Ak , Bk and I¯k , the areas of the bonded steel are transformed into equivalent areas of concrete by multiplying by the age-adjusted modular ratio n¯ es(i),k (= Es(i) /Ee,k ) or n¯ ep(i),k = (Ep(i) /Ee,k ), as appropriate. Based on Eqs 5.42, the expression for Fk (Eq. 5.40) can be re-written as: I¯k − Bk 1 Fk = Ee,k ( Ak I¯k − B2k ) − Ak Bk

(5.43)

The calculation of the time-dependent stresses and deformations using the above procedure is illustrated in Examples 5.3 and 5.4.

Example 5.3 For the reinforced concrete section shown in Fig. 5.5, the strain and stress distributions at τ0 immediately after the application of an axial force Ne,0 = −30 kN and a bending moment of Me,0 = 50 kNm were calculated in Example 5.1. If the applied loads remain constant during the time interval τ0 to τk , the strain and stress distributions at time τk are to be determined using the age-adjusted effective modulus method. As in Example 5.1, Ec,0 = 25 GPa; Es = 200 GPa; and ns,0 = Es /Ec,0 = 8. Take ϕ (τk , τ0 ) = 2.5; χ (τk , τ0 ) = 0.65; εsh (τk ) = −600 × 10−6 and assume the steel reinforcement is linear elastic. From Example 5.1: At τ0 : εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 25,000 = 9524 MPa = 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.5

and therefore n¯ es,k = 21.0; ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.5 × (0.65 − 1.0) = −0.333 Fe,0 = = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.5 The properties of the concrete part of the cross-section are: Ac = bD − As(1) − As(2) = 300 × 600 − 620 − 1800 = 177,600 mm2 Bc = bD(D/2 − dref ) − As(1) ys(1) − As(2) ys(2) = 300 × 600 × (300 − 200) − 620 × (−150) − 1800 × 350 = 17.46 × 106 mm3

2 bD3 D 300 × 6003 2 2 Ic = + bD − dref − As(1) ys(1) − As(2) ys(2) = 12 2 12 + 300 × 600 × (300 − 200)2 − 620 × (−150)2 − 1800 × 3502 = 6966 × 106 mm4

158 Uncracked sections and the properties of the age-adjusted transformed cross-section are: Ak = bD + (n¯ es,k − 1)[As(1) + As(2) ] = 300 × 600 + (21 − 1) × [620 + 1800] = 228,400 mm2

D Bk = bD − dref + (n¯ es,k − 1)[As(1) ys(1) + As(2) ys(2) ] = 300 × 600 2 × (300 − 200) + (21 − 1) × [620 × (−150) + 1800 × 350] = 28.74 × 106 mm3

2 3 ¯Ik = bD + bD D − dref + (n¯ es,k − 1)[As(1) y2 + As(2) y2 ] s(1) s(2) 12 2 300 × 6003 + 300 × 600 × (300 − 200)2 + 20 × [620 × (−150)2 12

=

+ 1800 × 3502 ] = 11,890 × 106 mm4 From Eq. 5.36: ⎤ ⎡ 177,600 × −42.7 × 10−6 + 17.46 × 106 ⎥ ⎢ ×0.331 × 10−6 ⎥ ⎢ fcr.k = −0.333 × 25,000 × ⎢ ⎥ ⎣17.46 × 106 × −42.7 × 10−6 + 6966 × 106 ⎦ ×0.331 × 10−6 =

+14.9 × 103 N

−13.0 × 106 Nmm

and from Eq. 5.37: 177,600 × 9524 × −600 × 10−6 −1015 × 103 N = fsh,k = −99.79 × 106 Nmm 17.46 × 106 × 9524 × −600 × 10−6

Eq. 5.43 gives: Fk =

1 9524 × (228,400 × 11,890 × 106 − (28.74 × 106 )2 ) 11,890 × 106 −28.74 × 106 × −28.74 × 106 228,400

=

660.7 × 10−12 N−1

−1.597 × 10−12 N−1 mm−1

−1.597 × 10−12 N−1 mm−1

12.69 × 10−15 N−1 mm−2

Uncracked sections 159 The strain εk at time τk is determined using Eq. 5.39: εk = Fk (re,k − fcr,k + fsh,k ) 660.7 × 10−12 −1.597 × 10−12 (−30 − 14.9 − 1015) × 103 = −1.597 × 10−12 12.69 × 10−15 (50 + 13.0 − 99.79) × 106 −641.4 × 10−6 = +1.226 × 10−6 mm−1 That is, the strain at the reference axis and the curvature at time τk are εr,k = −641.4 × 10−6 and κk = +1.226 × 10−6 mm−1 , respectively, and from Eq. 5.1, the top (y = −200 mm) and bottom (y = +400 mm) ﬁbre strains are: εk(top) = εr,k + (−200) × κk = (−641.4 − 200 × 1.226) × 10−6 = −886.5 × 10−6 and εk(btm) = εr,k +400×κk = (−641.4+400×1.226)×10−6 = −151.1×10−6 The concrete stress distribution at time τk is calculated using Eq. 5.41a: σc,k(top) = 9524

! −641.4 × 10−6 −6 1 −200 − (−600 × 10 ) +1.226 × 10−6

+ (−0.333) (−2.27) = −1.82 MPa ! −641.4 × 10−6 −6 σc,k(btm) = 9524 1 400 − (−600 × 10 ) +1.226 × 10−6 + (−0.333) (2.25) = 3.52 MPa and, from Eq. 5.42b, the stresses in the reinforcement are:

−641.4 × 10−6 +1.226 × 10−6

3

1 −150

3

−641.4 × 10−6 1 350 +1.226 × 10−6

σs(1),k = Es(1) 1 ys(1) εk = 200 × 10 = −165 MPa and

σs(2),k = Es(2) 1 ys(2) εk = 200 × 10 = −42.5 MPa

160 Uncracked sections The stress and strain distributions at τo (from Example 5.1) and at τk are shown in Fig. 5.11. time, t0 time, tk −886.5

−2.72 −1.82 −165 −18.5

−108.9

x

σ

e 0.331 × 10 −6

1.226 × 10

−6

mm

−1

mm

−42.5 14.6 −151.1

y

89.8

(b) Strain (× 10−6)

(a) Cross-section

−1

2.25 3.52 (c) Stress (MPa)

Figure 5.11 Strain and stress diagrams for Example 5.3 (all units in mm, MPa).

The cross-sectional rigidities could also have been calculated based on Eqs 5.30 and 5.32 without modifying the geometry of the section as: Ee,k + RA,k = Ac

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) = Ac Ec0 + As(1) + As(2) Es

i=1

6

= 2175 × 10 N; Ee,k + RB,k = Bc

ms

ys(i) As(i) Es(i) +

mp

i=1

yp(i) Ap(i) Ep(i)

i=1

= Bc Ee,k + As(1) ys(1) + As(2) ys(2) Es = 273.7 × 109 Nmm; and Ee,k + RI,k = Ic

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

i=1

2 2 = Ic Ee,k + As(1) ys(1) + As(2) ys(2) Es = 113.2 × 1012 Nmm2 . Fk is then determined using Eq. 5.40 (and is identical to that calculated earlier using Eq. 5.43):

RI,k −RB,k 1 Fk = RA,k RI,k − R2B,k −RB,k RA,k =

1

2 273.7 × 109 −273.7 × 109 2175 × 106

2175 × 106 × 113.2 × 1012 −

×

113.2 × 1012 −273.7 × 109

660.7 × 10−12 N−1 −1.597 × 10−12 N−1 mm−1 = −1.597 × 10−12 N−1 mm−1 12.69 × 10−15 N−1 mm−2

Uncracked sections 161

Example 5.4 A time-dependent analysis of the prestressed concrete section of Example 5.2 (see Figure 5.7) is to be undertaken using the age-adjusted effective modulus method. The strain and stress distributions at τ0 immediately after the application of an axial force Ne,0 = −100 kN and a bending moment of Me,0 = −50 kNm were calculated in Example 5.2. If the applied loads remain constant during the time interval τ0 to τk , the strain and stress distributions at time τk are to be determined. As in Example 5.2: Ec,0 = 32 GPa; Es = Ep = 200 GPa; and therefore ns(i),0 = np(i),0 = 6.25. Take ϕ(τk , τ0 ) = 2.0; χ(τk , τ0 ) = 0.65; εsh (τk ) = −400 × 10−6 and, for the prestressing steel, ϕp (τk , τ0 , σp(i),init ) = 0.03. Assume the steel reinforcement is linear elastic. From Example 5.2 at τ0 : εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

32,000 = 13,910 MPa and therefore n¯ es,k = n¯ ep,k = 14.37 1 + 0.65 × 2.0

2.0 × (0.65 − 1.0) Fe,0 = = −0.304 1.0 + 0.65 × 2.0 The properties of the concrete part of the cross-section are: Ac = Agross − As(1) − As(2) − Ap(1) − Ap(2) = 312,700 mm2 Bc = Agross (dc − dref ) − [As(1) ys(1) + As(2) ys(2) ] − [Ap(1) yp(1) + Ap(2) yp(2) ] = 93.49 × 106 mm3 2 2 2 Ic = Igross + Agross (dc − dref )2 − [As(1) ys(1) + As(2) ys(2) ] − [Ap(1) yp(1) 2 + Ap(1) yp(1) ] = 76,960 × 106 mm4

and the properties of the age-adjusted transformed section in equivalent concrete areas are: Ak = Agross + (n¯ es,k − 1)[As(1) + As(2) ] + (n¯ ep,k − 1)[Ap(1) + Ap(2) ] = 374.5 × 103 mm2 Bk = Agross (dc − dref ) + (n¯ es,k − 1)[As(1) ys(1) + As(2) ys(2) ] + (n¯ ep,k − 1)[Ap(1) yp(1) + Ap(2) yp(2) ] = 125.7 × 106 mm3 2 2 I¯k = Igross + Agross (dc − dref )2 + (n¯ es,k − 1)(As(1) ys(1) + As(2) ys(2) ) 2 2 + Ap(2) yp(2) ) = 103.5 × 109 mm4 + (n¯ ep,k − 1)(Ap(1) yp(1)

162 Uncracked sections Eqs 5.36 and 5.37 give: +567.9 × 103 N fcr.k = +354.6 × 106 Nmm

and −1740 × 103 N fsh,k = −520 × 106 Nmm

and from Eq. 5.38a (and Example 5.2) and Eq. 5.38b: fp,init =

2000 × 103 N

1290 × 106 Nmm

and fp.rel,k =

2000 × 103 × 0.03

1290 × 106 × 0.03

=

60 × 103 N

38.7 × 106 Nmm

Using Eq. 5.43:

−393.1 × 10−15 N−1 mm−1 323.8 × 10−12 N−1 Fk = −393.1 × 10−15 N−1 mm−1 1.171 × 10−15 N−1 mm−2

and the strain vector εk at time τk is determined using Eq. 5.39: 323.8 × 10−12 −393.1 × 10−15 εk = −393.1 × 10−15 1.171 × 10−15 (−100 − 567.9 − 1740 − 2000 + 60) × 103 × (−50 − 354.6 − 520 − 1290 + 38.7) × 106 −552.5 × 10−6 = −0.840 × 10−6 mm−1

The strain at the reference axis and the curvature at time τk are therefore εr,k = −552.5 × 10−6 and κk = −0.840 × 10−6 mm−1 , respectively. From Eq. 5.1, the top (y = −300 mm) and bottom (y = +850 mm) ﬁbre strains are: εk(top) = εr,k + (−300) × κk = −300.5 × 10−6 and εk(btm) = εr,k + 850 × κk = −1266 × 10−6

Uncracked sections 163 The concrete stress distribution at time τk is calculated using Eq. 5.41a: ! −552.5 × 10−6 −6 σc,k(top) = 13,913 1 −300 − (−400 × 10 ) −0.840 × 10−6 + (−0.304) (1.45) = 0.94 MPa ! −552.5 × 10−6 −6 σc,k(btm) = 13,913 1 850 − (−400 × 10 ) −0.840 × 10−6 + (−0.304) (−12.8) = −8.16 MPa and, from Eq. 5.41b, the stresses in the non-prestressed reinforcement are: −552.5 × 10−6 3 σs(1),k = Es(1) 1 ys(1) εk = 200 × 10 1 −240 −0.840 × 10−6 = −70.2 MPa and

3

σs(2),k = Es(2) 1 ys(2) εk = 200 × 10

−552.5 × 10−6 1 790 −0.840 × 10−6

= −243.3 MPa From Example 5.2, the initial strains in the prestress before transfer are εp(1),init = εp(2),init = 0.00625 and the relaxation strains are therefore εp.rel(1),k = εp.rel(2),k = 0.00625 × 0.03 = 187.5 × 10−6 . The stresses in the prestressing tendons at τk are obtained from Eq. 5.41c: −552.5 × 10−6 σp(1),k = 200,000 × [1 580] + 0.00625 − 0.0001875 −0.840 × 10−6 = 1004 MPa and

−552.5 × 10−6 σp(2),k = 200,000 × [1 710] + 0.00625 − 0.0001875 −0.840 × 10−6 = 982 MPa

The changes in stress in each prestressing tendon between ﬁrst loading and time τk are therefore σp(1),k = σp(1),0 −σp(1),k = 1191−1004 = 187 MPa and σp(2),k = σp(2),0 − σp(2),k = 1181 − 982 = 199 MPa and represent the time-dependent loss of prestress in each tendon, with σp(1),k being 15.7 per cent of the initial stress in Ap(1) immediately after transfer and σp(2),k being 16.8 per cent of the initial stress in Ap(2) .

164 Uncracked sections The stress and strain distributions at τ0 (from Example 5.2) and at τk are shown in Fig. 5.12. −300.5 45.5

0.94 + 1.45 4.5 s

kk = −0.840 × 10−6 mm−1

x

−70.2 e

Time, t0 Time, tk k0 = −0.387 × 10−6 mm−1 −243.3

−1266 −399.8 y (a) Cross-section (b) Strain diagram (× 10−6)

−75.3

1191 1004 1181 982

−12.8 −8.16 (c) Stress diagram (MPa)

Figure 5.12 Strain and stress distributions for Example 5.4.

The cross-sectional rigidities calculated using Eqs 5.30 and 5.32 are: RA,k = Ac Ee,k + As(1) + As(2) Es + Ap(1) + Ap(2) Ep = 5210 × 106 N RB,k = Bc Ee,k + As(1) ys(1) + As(2) ys(2) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 1748 × 109 Nmm 2 2 RI,k = Ic Ee,k + As(1) ys(1) Es + As(2) ys(2) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 1440 × 1012 Nmm2 and the matrix Fk could have been determined conveniently using Eq. 5.41.

5.5 Long-term analysis of reinforced and prestressed cross-sections using the step-by-step procedure The age-adjusted effective modulus method outlined in the previous section is a practical means to evaluate the time-dependent deformations and stresses on a reinforced or prestressed concrete section. It involves a single time interval, with stresses and deformations calculated at the beginning and end of the time interval, i.e. at τ0 and τk as shown in Fig. 5.9. The level of accuracy of the results depends on the type of stress and/or deformation history undergone by the concrete. For a more accurate representation of concrete behaviour, a more reﬁned method may be required, such as the step-by-step method (see Section 4.3) or the Dirichlet Series approximation (Ref. 4–5). The step-by-step procedure involves the time domain being discretised into a number of instants τj (with j = 0, . . . , k), as shown in Fig. 4.3, with the latter instant in time τk being the one at which the structural response is sought. Structural response is calculated at each time instant, in turn, with the solution at τj relying on the solutions obtained at the previous time instants. To achieve this, the concrete stresses calculated at each instant in time are stored for use in the subsequent analyses.

Uncracked sections 165 The steel reinforcement and prestressing tendons (if any) are again assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationships for the steel at any time τj are: σs(i),j = Es(i) εj σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j

(5.44a) (5.44b)

Following the approach outlined in Section 4.3.3, the constitutive relationship for the concrete at τj is given by Eq. 4.25 reproduced below: j−1

σc,j = Ec,j εj − εsh,j + Fe,j,i σc,i

(4.25)

i=0

and if the rectangular approximation of the integral-type creep law is adopted, the instantaneous elastic modulus of concrete Ec,j and the term Fe,j,i are given by Eqs 4.26a and b (reproduced below for ease of reference): Ec,j =

1 Jj,j

(4.26a)

and Fe,j,i =

Jj,i+1 − Jj,i Jj,j

(4.26b)

If the trapezoidal approximation is used for the numerical integration, the expressions for Ec,j and Fe,j,i are given in Eqs 4.26c–f. For ease of notation, the rectangular rule is considered in this chapter and used in the subsequent examples. With the proposed approach, k + 1 analyses must be carried out in order to yield the structural response at any time τk . For each time instant τj (with j = 0, . . . , k), the equations utilised in the cross-sectional analysis are obtained from considerations of equilibrium: ri,j = re,j

(5.45)

where ri,j and re,j are, respectively, the internal cross-sectional stress resultants and the external actions calculated at time τj , as follows:

Ni,j ri,j = Mi,j

(5.46a)

and

Ne,j re,j = Me,j

(5.46b)

where Ni,j and Mi,j depict the internal axial force and moment resisted by the crosssection at time τj , while Ne,j and Me,j represent the external applied actions.

166 Uncracked sections As already presented for the AEMM, the internal actions can be calculated by combining the contributions of the concrete, reinforcing steel and tendons. For example, the internal axial force resisted by the cross-section at τj can be expressed as: Ni,j = Nc,j + Ns,j + Np,j

(5.47)

The axial force in the concrete can be represented based on its constitutive relationship (Eq. 4.25) as: ⎡ ⎤ j−1 ⎣Ec,j εj − εsh,j + σc,j dA = Fe,j,i σc,i ⎦ dA Nc,j = Ac

Ac

i=0

= Ac Ec,j εr,j + Bc Ec,j κj − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

(5.48)

i=0

where the axial forces Nc,i resisted by the concrete at times τi (with i = 0, . . . , j − 1) are known (i.e. they have been calculated in previous time steps) at the beginning of the analysis at τj . The axial forces in the reinforcement and tendons can be evaluated from the constitutive relations (Eqs 5.44) as: Ns,j =

ms ms As(i) Es(i) εr,j + ys(i) As(i) Es(i) κj i=1

(5.49a)

i=1

mp

Np,j =

mp Ap(i) Ep(i) εr,j + yp(i) Ap(i) Ep(i) κj i=1

+

i=1

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.49b)

i=1

Substituting Eqs 5.48 and 5.49 into Eq. 5.47 produces: mp ms ms As(i) Es(i) + Ap(i) Ep(i) εr,j + Bc Ec,j + ys(i) As(i) Es(i) Ni,j = Ac Ec,j + i=1 mp

+

i=1

i=1

yp(i) Ap(i) Ep(i) κj − Ac Ec,j εsh,j +

i=1

+

mp

j−1

Fe,j,i Nc,i

i=0

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

i=1

= RA,j εr,j + RB,j κj − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

i=0

+

mp i=1

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.50)

Uncracked sections 167 and following the same procedure, the internal moment Mi,j at τj can be determined as: Mi,j = Bc Ec,j +

ms

ys(i) As(i) Es(i) +

i=1

j−1

yp(i) Ap(i) Ep(i) εr,j

mp

2 ys(i) As(i) Es(i) +

i=1

+

i=1

ms

+ Ic Ec,j +

mp

2 yp(i) Ap(i) Ep(i)

κj − Bc Ec,j εsh,j

i=1

Fe,j,i Mc,i +

i=0

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

i=1

= RB,j εr,j + RI,j κj − Bc Ec,j εsh,j +

j−1

Fe,j,i Mc,i

i=0

+

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(5.51)

i=1

The cross-sectional rigidities RA,j , RB,j and RI,j at time τj are deﬁned as: RA,j = Ac Ec,j +

ms

As(i) Es(i) +

i=1

RB,j = Bc Ec,j +

RI,j = Ic Ec,j +

ms

mp

Ap(i) Ep(i)

(5.52a)

i=1

ys(i) As(i) Es(i) +

mp

i=1

i=1

ms

mp

2 ys(i) As(i) Es(i) +

i=1

yp(i) Ap(i) Ep(i)

2 yp(i) Ap(i) Ep(i)

(5.52b)

(5.52c)

i=1

In the calculation of Mi,j in Eq. 5.51, the moment Mc,i resisted by the concrete component at time τi is calculated based on the solutions at each of the previous time instants: Mc,i =

Ac

yσc,i dA =

Ac

i−1 yEc,i εi − εsh,i + y Fe,i,n σc,n dA

= Bc Ec,i εr,i + Ic Ec,i κi − Bc Ec,i εsh,i +

n=0 i−1

Fe,i,n Mc,n

(5.53)

n=0

Following the approach outlined previously, the equilibrium equations at time τj can then be written as: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j

(5.54)

168 Uncracked sections where

εr,j εj = κj

RA,j RB,j Dj = RB,j RI,j fcr,j =

j−1

(5.55a) (5.55b)

Fe,j,i rc,i

(5.55c)

i=0

fsh,j = fp,init =

Ac Ec,j εsh,j Bc mp Ap(i) Ep(i) εp(i),init

(5.55d)

(5.55e)

yp(i) Ap(i) Ep(i) εp(i),init

i=1

fp.rel,j = fp,init ϕp (τj , σp(i),init )

(5.55f)

To simplify the notation, the internal actions resisted by the concrete at a previous time instant τi (calculated from Eqs 5.48 and 5.53) are collected in vector rc,i and expressed as:

i−1 Nc,i Ac Ec,i rc,i = = Dc,i εi + Fe,i,n rc,n − ε = Dc,i εi + fcr,i − fsh,i Mc,i Bc Ec,i sh,i

(5.56)

n=0

with

Ac Bc Dc,i = Ec,i Bc Ic

(5.57)

The strain vector εj at time τj is obtained by solving Eq. 5.54 and, as in the analyses presented earlier: εj = D−1 re,j − fcr,j + fsh,j − fp,init + fp.rel,j = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j j (5.58) in which Fj =

1 RA,j RI,j − R2B,j

RI,j −RB,j −RB,j RA,j

(5.59)

Finally, the stress distributions at time, τj , can be determined from the constitutive relationships (Eqs 5.44 and 4.25): σc,j = Ec,j εj − Ec,j εsh,j +

j−1 i=0

j−1

Fe,j,i σc,i = Ec,j

& ' 1 y εj − εsh,j + Fe,j,i σc,i i=0

(5.60a)

Uncracked sections 169

σs(i),j = Es(i) εj = Es(i) 1 yp(i) εj σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j = Ep(i) 1 yp(i) εj + Ep(i) εp(i),init − Ep(i) εp.rel(i),j

(5.60b)

(5.60c)

where εj = εr,j + yκj = 1 y εj . The cross-sectional rigidities at time τj , RA,j , RB,j and RI,j , can also be calculated from the properties of the transformed cross-section as follows: RA,j = Aj Ee,j

(5.61a)

RB,j = Bj Ee,j

(5.61b)

RI,j = Ij Ee,j

(5.61c)

where Aj , Bj and Ij are the area and the ﬁrst and second moments of the area, respectively, of the transformed section about the reference axis. For the transformed section, the area of the reinforcement and bonded tendons are usually transformed into equivalent areas of concrete, based on Ec,j using modular ratios of ns(i),j (= Es(i) /Ec,j ) for the bonded steel reinforcement and np(i),j (= Ep(i) /Ec,j ) for the bonded tendons. The matrix F0 in Eq. 5.58 can then be calculated as:

Ij Fj = 2 −B Ee,j (Aj Ij − Bj ) j 1

−Bj Aj

(5.62)

In the following two examples, Examples 5.3 and 5.4 are re-analysed using the step-by-step method.

Example 5.5 For the reinforced concrete section shown in Fig. 5.5 (and analysed previously in Examples 5.1 and 5.3), determine the stress distribution at 30,000 days after ﬁrst loading (i.e. approx. 80 years) using the step-by-step procedure. The external loading is applied at time τ0 = 28 days and kept constant over time (i.e. Ne,j = −30 kN and Me,j = 50 kNm). A very coarse time discretisation is adopted in this example to illustrate all the steps involved in the solution process. The time period is subdivided into two intervals, τ0 to τ1 and τ1 to τ2 , where τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. In structural design, a ﬁner discretisation is usually adopted to obtain more accurate results. For convenience in this example, shrinkage is assumed to begin at the time of ﬁrst loading (i.e. at τ0 ). The reinforcement is assumed to be linear-elastic. The relevant properties of the concrete are as follows: Ec,0 = 25 GPa; Ec,1 = 28 GPa; Ec,2 = 30 GPa; ϕ (τ0 , τ0 ) = 0; ϕ (τ1 , τ0 ) = 1.5; ϕ (τ2 , τ0 ) = 2.5; ϕ (τ1 , τ1 ) = 0; ϕ (τ2 , τ1 ) = 2.0; εsh (τ0 ) = εsh,0 = 0; εsh (τ1 ) = εsh,1 = −300 × 10−6 ; and εsh (τ2 ) = εsh,2 = −600 × 10−6 .

170 Uncracked sections Usually when using the step-by-step method (SSM), it is convenient to calculate the material properties for the concrete at the beginning of the analysis. From Eqs 1.10 and 4.26a and b: J (τ0 , τ0 ) =

1 1 = = 4 × 10−5 MPa−1 Ec,0 25,000

J (τ1 , τ1 ) =

1 1 = = 3.571 × 10−5 MPa−1 Ec,1 28,000

J (τ2 , τ2 ) =

1 1 = = 3.333 × 10−5 MPa−1 Ec,2 30,000

J (τ1 , τ0 ) =

1 + ϕ (τ1 , τ0 ) 1 + 1.5 = = 10 × 10−5 MPa−1 Ec,0 25,000

J (τ2 , τ0 ) =

1 + ϕ (τ2 , τ0 ) 1 + 2.5 = = 14 × 10−5 MPa−1 Ec,0 25,000

J (τ2 , τ1 ) =

1 + ϕ (τ2 , τ1 ) 1 + 2.0 = = 10.71 × 10−5 MPa−1 Ec,1 28,000

Fe,1,0 =

J (τ1 , τ1 ) − J (τ1 , τ0 ) = −1.8 J (τ1 , τ1 )

Fe,2,0 =

J (τ2 , τ1 ) − J (τ2 , τ0 ) = −0.986 J (τ2 , τ2 )

Fe,2,1 =

J (τ2 , τ2 ) − J (τ2 , τ1 ) = −2.214 J (τ2 , τ2 )

Considering that the externally applied actions remain constant with time and the problem involves no prestressing tendons (for j = 0, 1 and 2):

−30 × 103 N re,j = 50 × 106 Nmm

0N fp,init = 0 Nmm

0N fp.rel,j = 0 Nmm

Short-term analysis (τ0 = 28 days) From Example 5.1: εr,0 = −42.7 × 10−6 and κ0 = 0.331 × 10−6 mm−1 . From Example 5.3: Ac = 177.6 × 103 mm2 , Bc = 17.46 × 106 mm3 and Ic = 6966 × 106 mm4 .

Uncracked sections 171 The stress resultants resisted by the concrete at τ0 are determined from Eq. 5.56: rc,0 = Dc,0 ε0 + fcr,0 − fsh,0 177.6 × 103 17.46 × 106 −42.7 × 10−6 0 0 = 25,000 × + − −6 6 6 0 0 0.331 × 10 17.46 × 10 6966 × 10 −44.9 × 103 N = 39.1 × 106 Nmm

Time analysis – SSM (τ1 = 100 days) – time step 1: Considering Ec,1 for the concrete component, the cross-sectional rigidities at time τ1 can be determined from Eqs 5.52 as: RA,1 = 5456 × 106 N RB,1 = 596.4 × 109 Nmm RI,1 = 241.9 × 1012 Nmm2 from which D1 and F1 can be determined (Eqs 5.55b and 5.59) as:

5456 × 106 N 596.4 × 109 Nmm RA,1 RB,1 D1 = = RB,1 RI,1 596.4 × 109 Nmm 241.9 × 1012 Nmm2 and F1 =

1

RI,1 −RB,1 −RB,1 RA,1

RA,1 RI,1 − R2B,1 −618.4 × 10−15 N−1 mm−1 250.8 × 10−12 N−1 = −618.4 × 10−15 N−1 mm−1 5.658 × 10−15 N−1 mm−2

Creep effects due to the initial concrete stresses and shrinkage effects are obtained from Eq. 5.55c and d: 80.8 × 103 N −44.9 × 103 fcr,1 = Fe,1,0 rc,0 = −1.8 × = 39.1 × 106 −70.3 × 106 Nmm and

Ac 177.6 × 103 fsh,1 = Ec,1 εsh,1 = × 28,000 × −300 × 10−6 6 Bc 17.46 × 10 −1492 × 103 N = −146.7 × 106 Nmm

172 Uncracked sections The strain distribution at time τ1 becomes (Eq. 5.58): ε1 = F1 re,1 − fcr,1 + fsh,1 250.8 × 10−12 −618.4 × 10−15 = −618.4 × 10−15 5.658 × 10−15 −30 × 103 80.8 × 103 −1492 × 103 × − + 50 × 106 −70.3 × 106 −146.7 × 106 −385.7 × 10−6 = 0.841 × 10−6 mm−1 Therefore, εr,1 = −385.7 × 10−6 and κ1 = 0.841 × 10−6 mm−1 and the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε1(top) = εr,1 + (−200) × κ1 = −554.0 × 10−6 and ε1(btm) = εr,1 + 400 × κ1 = −49.0 × 10−6 The top and bottom ﬁbre concrete stresses at time τ1 are (Eq. 5.60): σc,1(top) = Ec,1 σc,1(btm) = Ec,1

" 1 y

# ε − ε 1 sh,1 + Fe,1,0 σc,0(top) = −2.21 MPa c,(top) & ' 1 yc,(btm) ε1 − εsh,1 + Fe,1,0 σc,0(btm) = 2.98 MPa

and the stresses in the reinforcement are: σs(1),1 = Es(1) 1 ys(1) ε1 = −102.4 MPa σs(2),1 = Es(2) 1 ys(2) ε1 = −18.2 MPa Based on these results the axial force and moment resisted by the concrete component at time τ1 are (Eq. 5.56):

Ac Bc εr1 rc,1 = Dc,1 ε1 + fcr,1 − fsh,1 = Ec,1 + fcr,1 − fsh,1 Bc Ic κ1 −385.7 × 10−6 177.6 × 103 17.46 × 106 = 28,000 × 0.841 × 10−6 17.46 × 106 6966 × 106 80.8 × 103 −1492 × 103 + − −70.3 × 106 −146.7 × 106 66.3 × 103 N = 51.9 × 106 Nmm

Uncracked sections 173

Time analysis – SSM (τ2 = 30,000 days) – time step 2 The cross-sectional rigidities at time τ2 are (Eqs 5.52): RA,2 = 5811 × 106 N; RB,2 = 631.3 × 109 Nmm; RI,2 = 255.8 × 1012 Nmm2 . and from Eqs 5.55b and 5.59:

5811 × 106 N 631.3 × 109 Nmm D2 = 631.3 × 109 Nmm 255.8 × 1012 Nmm2 −580.0 × 10−15 N−1 mm−1 235.1 × 10−12 N−1 F2 = −580.0 × 10−15 N−1 mm−1 5.339 × 10−15 N−1 mm−2 The creep effects due to the concrete stresses in the previous time steps, at τ0 and τ1 , and the shrinkage effects are obtained from Eqs 5.55c and d:

−44.9 × 103 fcr,2 = Fe,2,0 rc,0 + Fe,2,1 rc,1 = −0.986 × 39.1 × 106 66.3 × 103 −102.5 × 103 N − 2.214 × = −153.5 × 106 Nmm 51.9 × 106

Ac 177.6 × 103 fsh,2 = Ec,2 εsh,2 = × 30,000 × −600 × 10−6 6 Bc 17.46 × 10 −3196 × 103 N = −314.3 × 106 Nmm The strain distribution at time τ2 can be calculated as (Eq. 5.58): ε2 = F2 re,2 − fcr,2 + fsh,2 =

−670.1 × 10−6 1.220 × 10−6 mm−1

With εr,2 = −670.1 × 10−6 and κ2 = 1.220 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε2(top) = εr,2 + (−200) × κ2 = −914.2 × 10−6 ε2(btm) = εr,2 + 400 × κ2 = −181.9 × 10−6

174 Uncracked sections The top and bottom ﬁbre concrete stresses at τ2 are (Eq. 5.60): σc,2(top) = Ec,2

" # 1 yc,(top) ε2 − εsh,2 + Fe,2,0 σc,0(top) + Fe,2,1 σc,1(top)

= 30,000

! −670.1 × 10−6 −6 1 −200 − −600 × 10 1.220 × 10−6

− 0.986 × (−2.72) − 2.214 × (−2.21) = −1.85 MPa " # 1 yc,(btm) ε2 − εsh,2 + Fe,2,0 σc,0(btm) + Fe,2,1 σc,1(btm) σc,2(btm) = Ec,2 = 3.72 MPa The ﬁnal stresses in the reinforcement are: σs(1),2 = Es(1) 1 ys(1) ε2 = −170.6 MPa σs(2),2 = Es(2) 1 ys(2) ε2 = −48.6 MPa The stress and strain distributions at τ0 and at τ2 are shown in Fig. 5.13. Time, t0 Time, t2 −914.2

−108.9

−2.72

−1.85 −18.5

−170.6

x

−6

−1

k0 = 0.331 × 10 mm

σ

e

kk = 1.220 × 10−6mm−1

−48.6 y

(a) Cross-section

−181.9 89.8 (b) Strain diagram (× 10−6)

14.6

2.25 3.72 (c) Stress diagram (MPa)

Figure 5.13 Initial and ﬁnal strain and stress diagrams for Example 5.5.

Example 5.6 For the prestressed cross-section shown in Fig. 5.7 and analysed in Examples 5.2 and 5.4, determine the stress distribution at 30,000 days using the stepby-step procedure. The sustained external actions, Ne,j = −100 kN and Me,j = −50 kNm are applied at time τ0 = 28 days and kept constant with time. As for Example 5.5, the time domain is discretised into two time steps, from τ0 to τ1 and from τ1 to τ2 , with τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. The reinforcement is assumed to be linear-elastic and the relevant properties of

Uncracked sections 175 the concrete are: Ec,0 = 32 GPa; Ec,1 = 36 GPa; Ec,2 = 40 GPa; ϕ (τ0 , τ0 ) = 0; ϕ (τ1 , τ0 ) = 1.0; ϕ (τ2 , τ0 ) = 2.0; ϕ (τ1 , τ1 ) = 0; ϕ (τ2 , τ1 ) = 1.5; εsh (τ0 ) = εsh,0 = 0; εsh (τ1 ) = εsh,1 = −200 × 10−6 ; and εsh (τ2 ) = εsh,2 = −400 × 10−6 . The initial strains in the prestressing tendons prior to transfer is εp(1),init = εp(2),init = 0.00625 and the creep coefﬁcient for the prestressing steel is ϕp (τ1 , σp,init ) = 0.02 and ϕp (τ2 , σp,init ) = 0.03. The relevant creep functions for concrete are (Eqs 1.10 and 4.26a and b): J (τ0 , τ0 ) = 3.125 × 10−5 MPa−1 J (τ1 , τ1 ) = 2.777 × 10−5 MPa−1 J (τ2 , τ2 ) = 2.5 × 10−5 MPa−1 J (τ1 , τ0 ) = 6.25 × 10−5 MPa−1 J (τ2 , τ0 ) = 9.375 × 10−5 MPa−1 J (τ2 , τ1 ) = 6.944 × 10−5 MPa−1 Fe,1,0 = −1.25 Fe,2,0 = −0.972 Fe,2,1 = −1.777 Considering that the externally applied actions remain constant with time, for j = 0, 1 and 2: −100 × 103 N re,j = −50 × 106 Nmm

and 2000 × 103 N fp,init = 1290 × 106 Nmm

Short-term analysis (τ0 = 28 days) From Example 5.2: εr,0 = −70.7 × 10−6 and κ0 = −0.387 × 10−6 mm−1 . From Example 5.4: Ac = 312.7 × 103 mm2 ; Bc = 93.49 × 106 mm3 ; Ic = 76,960 × 106 mm4 . From Eq. 5.56, the stress resultants resisted by the concrete at τ0 are:

Ac Bc εr,0 0 0 rc,0 = Dc,0 ε0 + fcr,0 − fsh,0 = Ec,0 + − Bc Ic κ0 0 0 −1865 × 103 N = −1165 × 106 Nmm

176 Uncracked sections

Time analysis – SSM (τ1 = 100 days) – time step 1 From Eqs 5.52, the cross-sectional rigidities at time τ1 are: RA,1 = 12,120 × 106 N RB,1 = 3813 × 109 Nmm RI,1 = 3140 × 1012 Nmm2 and from Eq. 5.59:

133.6 × 10−12 N−1 mm−2 −162.2 × 10−15 N−1 mm−1 F1 = −162.2 × 10−15 N−1 mm−1 515.4 × 10−18 N−1

The effects of creep due to the concrete stresses calculated at τ0 and the effects of shrinkage are represented as: 2332 × 103 N −1865 × 103 fcr,1 = Fe,1,0 rc,0 = −1.25 × = 1456 × 106 Nmm −1165 × 106

Ac 312.7 × 103 −6 fsh,1 = Ec,1 εsh,1 = × 36,000 × −200 × 10 Bc 93.46 × 106 −2251 × 103 N = −673.2 × 106 Nmm

and the relaxation of the prestressing tendons is: fp.rel,1 =

Ap(1) Ep(1) εp(1),init

ϕp (τ1 , σp(1),init ) yp(1) Ap(1) Ep(1) εp(1),init Ap(2) Ep(2) εp(2),init + ϕp (τ1 , σp(2),init ) yp(2) Ap(2) Ep(2) εp(2),init

800 × 200,000 × 0.00625 = × 0.02 580 × 800 × 200,000 × 0.00625

800 × 200,000 × 0.00625 + × 0.02 710 × 800 × 200,000 × 0.00625 40 × 103 N = 25.8 × 106 Nmm

Uncracked sections 177 The strain distribution at time τ1 becomes: ε1 = F1 re,1 − fcr,1 + fsh,1 − fp,init + fp.rel,1 133.6 × 10−12 −162.2 × 10−15 = −162.2 × 10−15 515.4 × 10−18 −100 × 103 2332 × 103 −2251 × 103 × − + −50 × 106 1456 × 106 −673.2 × 106 2000 × 103 40 × 103 −328.8 × 10−6 − + = 1290 × 106 25.8 × 106 −0.697 × 10−6 mm−1 With εr,1 = −328.8 × 10−6 and κ1 = −0.697 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε1(top) = εr,1 + (−300) × κ1 = −119.6 × 10−6 and ε1(btm) = εr,1 + 850 × κ1 = −921.6 × 10−6 . The stresses in the top and bottom concrete ﬁbres at time τ1 are (Eqs 5.60): " # 1 yc,(top) ε1 − εsh,1 + Fe,1,0 σc,0(top) = 1.07 MPa σc,1(top) = Ec,1 & ' σc,1(btm) = Ec,1 1 yc,(btm) ε1 − εsh,1 + Fe,1,0 σc,0(btm) = −9.98 MPa and the stress in the non-prestressed reinforcement is:

3

−328.8 × 10−6 1 −240 −0.697 × 10−6

3

−328.8 × 10−6 1 790 −0.697 × 10−6

σs(1),1 = Es(1) 1 ys(1) ε1 = 200 × 10 = −32.3 MPa

σs(2),1 = Es(2) 1 ys(2) ε1 = 200 × 10 = −176.0 MPa

The stress in the prestressing steel is: σp(1),1 = Ep(1) 1 yp(1) ε1 + Ep(1) εp(1),init − εp.rel(1),1 −328.8 × 10−6 3 1 580 = 200 × 10 −0.697 × 10−6 + 200 × 103 × 0.00625 × (1 − 0.02) = 1078 MPa σp(2),1 = Ep(2) 1 yp(2) ε1 + Ep(2) εp(2),init − εp.rel(2),1 = 1060 MPa

178 Uncracked sections The axial force and moment resisted by the concrete component at time τ1 are (Eq. 5.56):

Ac Bc εr1 rc,1 = Dc,1 ε1 + fcr,1 − fsh,1 = Ec,1 + fcr,1 − fsh,1 Bc Ic κ1 −1465 × 103 N = −909.3 × 106 Nmm

Time analysis – SSM (τ2 = 30,000 days) – time step 2 The cross-sectional rigidities at time τ2 are (Eqs 5.52): RA,2 = 13,370 × 106 N RB,2 = 4187 × 109 Nmm RI,2 = 3448 × 1012 Nmm2 120.7 × 10−12 N−1 mm−2 −146.6 × 10−15 N−1 mm−1 F2 = −146.6 × 10−15 N−1 mm−1 468.1 × 10−18 N−1 Creep effects due to the concrete stresses in previous time steps, i.e. at τ0 and τ1 , are: fcr,2 = Fe,2,0 rc,0 + Fe,2,1 rc,1 −1465 × 103 −1865 × 103 = −0.972 × − 1.777 × −1165 × 106 −909.3 × 106 4418 × 103 N = 2749 × 106 Nmm and shrinkage effects are:

Ac 312.7 × 103 fsh,2 = Ec,2 εsh,2 = × 40,000 × −400 × 10−6 6 Bc 93.49 × 10 −5003 × 103 N = −1496 × 106 Nmm The relaxation of the prestressing tendons is: Ap(1) Ep(1) εp(1),init fp.rel,2 = ϕp (τ2 , σp(1),init ) yp(1) Ap(1) Ep(1) εp(1),init Ap(2) Ep(2) εp(2),init 60 × 103 N + ϕp (τ2 , σp(2),init ) = 38.7 × 106 Nmm yp(2) Ap(2) Ep(2) εp(2),init

Uncracked sections 179 The strain distribution at time τ2 is: ε2 = F2 re,2 − fcr,2 + fsh,2 − fp,init + fp.rel,2 =

−570.6 × 10−6 −0.915 × 10−6 mm−1

With εr,2 = −570.6 × 10−6 and κ2 = −0.915 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε2(top) = εr,2 + (−300) × κ2 = −295.8 × 10−6 and ε2(btm) = εr,2 + 850 × κ2 = −1349 × 10−6 The stresses in the top and bottom concrete ﬁbres at time τ1 are (Eqs 5.60): " # 1 yc,(top) ε2 − εsh,2 + Fe,2,0 σc,0(top) + Fe,2,1 σc,1(top) ! −570.6 × 10−6 −6 = 40,000 1 −300 − −400 × 10 −0.915 × 10−6

σc,2(top) = Ec,2

− 0.972 × 1.45 − 1.777 × 1.07 = 0.84 MPa " # 1 yc,(btm) ε2 − εsh,2 + Fe,2,0 σc,0(btm) + Fe,2,1 σc,1(btm) σc,2(btm) = Ec,2 = −7.77 MPa and the stresses in the non-prestressed reinforcement are:

3

−570.6 × 10−6 1 −240 −0.915 × 10−6

3

−570.6 × 10−6 1 790 −0.915 × 10−6

σs(1),2 = Es(1) 1 ys(1) ε2 = 200 × 10 = −70.1 MPa

σs(2),2 = Es(2) 1 ys(2) ε2 = 200 × 10 = −258.8 MPa

The ﬁnal stresses in the prestressing tendons are: σp(1),2 = Ep(1) 1 yp(1) ε2 + Ep(1) εp(1),init − εp.rel(1),2 = 992.1 MPa σp(2),2 = Ep(2) 1 yp(2) ε2 + Ep(2) εp(2),init − εp.rel(2),2 = 968.3 MPa

180 Uncracked sections The stress and strain distributions at τ0 and at τ2 are shown in Fig. 5.14. −295.8 45.5 −70.1

k2 = −0.915 × 10−6 mm−1

x

0.84 1.45 4.5

e

s

Time, t0 Time, t2

−6

k0 = −0.387 × 10 mm

−1349

y

−399.8

(b) Strain diagram (×

(a) Cross-section

−258.8

−1

−12.8

10−6)

−75.3

992.1 968.3

1191 1181

−7.77

(c) Stress diagram (MPa)

Figure 5.14 Initial and ﬁnal strain and stress diagrams for Example 5.6.

5.6 Composite steel-concrete cross-sections The analysis of composite steel-concrete cross-sections, such as those shown in Fig. 5.15, is presented here. Each cross-section has a single axis of symmetry and may be subjected to any combination of axial force and bending moment. In addition to the rolled or fabricated steel section or proﬁled decking, the concrete deck may contain layers of steel reinforcement. Mechanical shear connections are usually used to ensure that the steel-concrete interface is capable of carrying the imposed horizontal shear, and that the steel and concrete portions act compositely. For most practical steel-concrete composite sections, little slip occurs between the steel and the concrete under normal in-service conditions, with the magnitude of any slip depending on the rigidity of the interface connection (Refs 6–11). In the following, a perfect bond between the steel and the concrete is assumed.

..

.

.

.

.

.

.

.

.

. .

.

.

.

.

. . .

Steel reinforcement

Concrete . .. . . . . . . . . . . .. . . .. .. . . .. . . . . . . . . . . .. . . . . .. . . . . . . . . .

Steel

Concrete

Permanent steel formwork

Figure 5.15 Composite steel-concrete cross-sections.

Uncracked sections 181 The procedures for the short- and long-term analyses of the composite sections shown in Fig. 5.15 are similar to those presented for reinforced and prestressed concrete sections in Sections 5.3–5.5, except that the ﬂexural rigidity of the steel section (or its second moment of area) must be included, as well as its cross-sectional area. At any time instant τk , the internal axial force and moment resisted by the composite cross-section, Ni,k and Mi,k , respectively, may be expressed as: Ni,k = Nc,k + Ns,k + Nss,k

(5.63a)

Mi,k = Mc,k + Ms,k + Mss,k

(5.63b)

where Nc,k , Ns,k and Nss,k are the resultant axial forces in the concrete, the nonprestressed reinforcement and the steel part of the cross-section, respectively, and Mc,k , Ms,k and Mss,k are the corresponding moments about the reference axis. Since the rolled or fabricated steel (or permanent steel decking) does not creep or shrink, Nss,k and Mss,k may be deﬁned at any time τk as: Nss,k =

Ass

σss,k dA =

Ass

Mss,k =

Ass

Ess (εr,k + yκk ) dA = Ass Ess εr,k + Bs Ess κk

(5.64a)

yσss,k dA =

Ass

yEss (εr,k + yκk )d A = Bss Ess εr,k + Is Ess κk

(5.64b)

where Ass is the cross-sectional area of the rolled or fabricated steel section, and Bss and Iss are the ﬁrst and second moments of area of the steel section calculated with respect to the adopted reference axis. The constitutive relationship for the rolled or fabricated steel is assumed to be linear-elastic as follows: σss,k = Ess εk = Ess [1

y]εk

(5.65)

The advantage of this representation is that it describes both the instantaneous analysis (at τ0 ) and the time-dependent analysis (at τk ). At k = 0, Eqs 5.63 can be substituted into Eqs 5.2 to produce the governing equilibrium equations for a short-term analysis (as previously presented in Eq. 5.12). Using the AEMM for the time analysis (at τk ), Eqs 5.63 can be substituted into Eq. 5.24 to obtain the governing equations (previously presented in Eqs 5.34). The solution using the SSM is obtained by replacing Eqs 5.47 and 5.51 with Eqs 5.63 (and with time τj used instead of τk ). The only differences between the analyses of the composite steel-concrete crosssection and the analyses presented in Sections 5.3–5.5 are in the calculation of the cross-sectional rigidities, RA,k , RB,k and RI,k . The solution processes, involving the determination of the unknown strain and stress distributions at τk , are unchanged. For a composite steel-concrete cross-section, using the AEMM, the cross-sectional rigidities are: Ee,k + Ass Ess + RA,k = Ac

ms i=1

As(i) Es(i)

(5.66a)

182 Uncracked sections RB,j = Bc Ee,j + Bss Ess +

ms

ys(i) As(i) Es(i)

(5.66b)

i=1

Ee,j + Iss Ess + RI,j = Ic

ms

2 ys(i) As(i) Es(i)

(5.66c)

i=1

Ee,k = Ec,0 . When using the SSM, the concrete where for the short-term analysis at τ0 , modulus to be used in Eq. 5.66 is the one associated with the time step under consideration. As already discussed for reinforced and prestressed concrete sections, it is also common to transform the steel parts of the cross-section into equivalent areas of concrete, to calculate the rigidities of the transformed concrete section, and to use these in the analysis instead of the rigidities calculated using Eq. 5.66.

Example 5.7 The short-term and ﬁnal long-term behaviour of the composite cross-section shown in Fig. 5.16 is to be calculated. The cross-section is subjected to a sustained bending moment Me = 500 kNm. The axial force Ne in this example is zero. The time-dependent behaviour of the concrete is to be modelled using the AEMM and the relevant material properties are: Ec,0 = 25,000 MPa Ess = Es(1) = 200,000 MPa ϕ0∗ = ϕ (∞, τ0 ) = 2.5 χ0∗ = χ (∞, τ0 ) = 0.65 ∗ = εsh (∞) = −600 × 10−6 εsh

2400 75 75

150 dref = 450 x

600

y

As(1) = 2700 mm2 ys(1) = −375

Ass = 12,500 mm2 Iss = 750 μ 106 mm2 Centroid of Ass located at dref

Figure 5.16 Cross-sectional details for Example 5.7 (all dimensions in mm).

Uncracked sections 183 The external actions remain constant with time and are given by (with j = 0, k)

0N Ne,j = re,j = Me,j 500 × 106 Nmm

Short-term analysis (at time τ0 ) The geometric properties of the concrete slab are: Ac = bD−As(1) = 2400×150−2700 = 357,300 mm2 Bc = bD(D/2−dref )−As(1) ys(1) = 2400×150×(75−450)−2700×(−375) = −134.0×106 mm3

2 bD3 2400×1503 D 2 Ic = = +bD −dref −As(1) ys(1) 12 2 12 +2400×150×(75−450)2 −2700×(−375)2 = 50,920×106 mm4 The properties of the steel beam are already provided with respect to dref : Ass = 12,500 mm2 ; Bss = 0 mm3 (as the centroid of the steel beam is located on the reference axis); and Iss =750×106 mm4 . The cross-sectional rigidities are calculated using Eqs 5.66: RA,0 = Ac Ec,0 + Ass Ess +

ms

As(i) Es(i) = Ac Ec,0 + Ass Ess + As(1) Es(1)

i=1

= 11,970 × 106 N RB,0 = Bc Ec,0 + Bss Ess +

ms

ys(i) As(i) Es(i) = Bc Ec,0 + Bss Ess + ys(1) As(1) Es(1)

i=1 9

= −3552 × 10 Nmm RI,0 = Ic Ec,0 + Iss Ess +

ms

2 2 ys(i) As(i) Es(i) = Ic Ec,0 + Iss Ess + ys(1) As(1) Es(1)

i=1 12

= 1499 × 10 From Eq. 5.15: F0 = =

1

Nmm2

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 2.81 × 10−10 N−1

6.66 × 10−13 N−1 mm−1

6.66 × 10−13 N−1 mm−1 2.24 × 10−15 N−1 mm−2

184 Uncracked sections At time τ0 , before any creep or shrinkage has occurred, Eq. 5.14 reduces to: ε0 = F0 re,0 = =

2.81 × 10−10 6.66 × 10−13

6.66 × 10−13 2.24 × 10−15 333.3 × 10−6

0 500 × 106

1.123 × 10−6 mm−1

With εr,0 = 333.3 × 10−6 and κ0 = 1.123 × 10−6 mm−1 , the strains at the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): ε0(top) = εr,0 + (−450) × κ0 = −172.2 × 10−6 and ε0(btm) = εr,0 + 300 × κ0 = 670.4 × 10−6 The concrete stresses at the top and bottom of the slab at time τ0 are (Eq. 5.16a):

σc,0(top) = Ec,0 1 yc,(top)

333.3 × 10−6 ε0 = 25,000 1 −450 1.123 × 10−6

= −4.31 MPa σc,0(btm) = Ec,0

333.3 × 10−6 1 yc,(btm) ε0 = 25,000 1 −300 1.123 × 10−6

= −0.09 MPa The stress in the steel reinforcement is (Eq. 5.16b):

3

σs(1),0 = Es(1) 1 ys(1) ε0 = 200 × 10

333.3 × 10−6 1 −375 1.123 × 10−6

= −17.6 MPa The stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65): ! 333.3×10−6 & ' 3 1 −300 σss,0(top) = Ess 1 yss,(top) ε0 = 200×10 1.123×10−6 = −0.74 MPa

! " # −6 333.3×10 σss,0(btm) = Ess 1 yss,(btm) ε0 = 200×103 1 +300 1.123×10−6 = 134 MPa

Uncracked sections 185 The stress resultants resisted by the concrete at τ0 can be determined from:

Nc,0 Ac Bc εr,0 −785.8 × 103 N rc,0 = = = Dc,0 ε0 = Ec,0 313.6 × 106 Nmm Bc Ic κ0 Mc,0

Time analysis – AEMM (at time τk = ∞) From Eqs 4.35 and 4.46: Ee,k =

25,000 = 9524 MPa 1 + 0.65 × 2.5

2.5 × (0.65 − 1.0) Fe,0 = = −0.333 1.0 + 0.65 × 2.5 The cross-sectional rigidities at time τk are (Eq. 5.66): RA,k = Ac Ee,k + Ass Ess + As(1) Es(1) = 6443 × 106 N Ee,k + Bss Ess + ys(1) As(1) Es(1) = −1479 × 109 Nmm RB,k = Bc 2 Ee,k + Iss Ess + ys(1) As(1) Es(1) = 710.9 × 1012 Nmm2 RI,k = Ic

Fk is then obtained using Eq. 5.40: Fk =

1

RI,k −RB,k −RB,k RA,k

RA,k RI,k − R2B,k 2.96 × 10−10 N−1 6.17 × 10−13 N−1 mm−1 = 6.17 × 10−13 N−1 mm−1 2.69 × 10−15 N−1 mm−2

The creep effects at τk due to the concrete stresses calculated at τ0 are calculated using Eq. 5.36: 3 3 N 261.9 × 10 −785.8 × 10 fcr,k = = Fe,0 rc,0 = −0.333 × −104.6 × 106 Nmm 313.6 × 106

and the shrinkage effects are given by Eq. 5.37:

357,300 × 9524 Ac fsh,k = −600 × 10−6 Ee,k εsh,k = 6 Bc −134 × 10 × 9524 −2042 × 103 N = 765.6 × 106 Nmm

186 Uncracked sections From Eq. 5.39, the ﬁnal strain distribution at time τk is: εk = Fk re,k − fcr,k + fsh,k =

162.2 × 10−6

2.265 × 10−6 mm−1

With εr,k = 162.2 × 10−6 and κk = 2.265 × 10−6 mm−1 , the strains in the top and bottom ﬁbres of the cross-sections are (Eq. 5.1): εk(top) = εr,k + (−450) × κk = −856.9 × 10−6 εk(btm) = εr,k + 300 × κk = 841.6 × 10−6 The ﬁnal concrete stresses at the top and bottom of the slab at time τk are (Eq. 5.41a): & ' 1 yc,(top) εk − εsh,k + Fe,0 σc,0 ! 162.2 × 10−6 −6 − −600 × 10 = 9524 1 −450 2.265 × 10−6

σc,k(top) = Ee,k

− 0.333 × (−4.31) = −1.01 MPa " # 1 yc,(btm) εk − εsh,k + σc,k(btm) = Ee,k Fe,0 σc,0 = 0.82 MPa The ﬁnal stress in the steel reinforcement is (Eq. 5.41b):

3

σs(1),k = Es(1) 1 ys(1) εk = 200 × 10

162.2 × 10−6 1 −375 2.265 × 10−6

= −137.4 MPa and the ﬁnal stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65):

3

σss,k(top) = Ess 1 yss,(top) εk = 200 × 10

162.2 × 10−6 1 −300 2.265 × 10−6

= −103.4 MPa

σss,k(btm) = Ess 1 yss,(btm) εk = 200 × 103 = 168.3 MPa

162.2 × 10−6 1 300 2.265 × 10−6

Uncracked sections 187 The ﬁnal stress and strain distributions are illustrated in Fig. 5.17. −856.9

−172.2

−4.31 −1.01

−17.6

−137 −103

kk = 2.265 × 10−6 mm−1 e

x Time, t0 −6 −1 Time, tk k0 = 1.123 × 10 mm

−0.74 Steel stress

670.4 841.6

y (a) Cross-section

−6)

(b) Strain diagram (×10

−0.09 0.82 Concrete stress

s

134 168 (c) Stress diagram (MPa)

Figure 5.17 Stress and strain distributions due to Me = 500 kNm (Example 5.7).

As can be seen in Fig. 5.17, the effect of creep and shrinkage in the concrete portions of a composite section in positive bending is to substantially increase positive curvature with time. In this example, the initial curvature has approximately doubled (from κ0 = 1.123 × 10−6 mm−1 to κk = 2.265 × 10−6 mm−1 ). In addition, the concrete deck has been relieved of much of its initial compression, with tensile stress developing in the bottom concrete ﬁbres. The steel I-section therefore carries signiﬁcantly more of the external moment after a period of sustained loading. Both the tensile stresses in the bottom ﬁbres of the steel I-section and the compressive stresses in the top ﬁbres have increased substantially with time.

Example 5.8 In order to examine the effects of shrinkage on the behaviour of a composite section, the cross-section shown in Fig. 5.16 (and analysed in Example 5.7) is here re-analysed for the case when Me = 0 and Ne = 0. As in Example 5.7, the ﬁnal shrinkage is −600 × 10−6 . This unloaded situation is quite common in practice, for example near the supports of a simply-supported member or at the points of contraﬂexure in a continuous composite girder. Obviously, in the short-term, the section is unloaded, with zero deformation (εr,0 = 0 and κ0 = 0) and no external actions. As time increases, the concrete deck shrinks while being restrained by the steel I-section and by the bonded steel reinforcement. As for Example 5.7: Ee,k = 9524 MPa; Fe,0 = −0.333; Ac = 2 6 3 357,300 mm ; Bc = −134 × 10 mm ; Ic = 50,920 × 106 mm4 ; RA,k = 6443 × 106 N; RB,k = −1479 × 109 Nmm; RI,k = 710.9 × 1012 Nmm2 ; and Fk =

2.96 × 10−10 N−1

6.17 × 10−13 N−1 mm−1

6.17 × 10−13 N−1 mm−1 2.69 × 10−15 N−1 mm−2

188 Uncracked sections With no external loads and from Eqs 5.36 and 5.37:

0N re,0 = re,k = 0 Nmm

0N fcr,k = 0 Nmm −2042 × 103 N fsh,k = 765.6 × 106 Nmm The ﬁnal strain distribution at time τk becomes (Eq. 5.39): εk = Fk re,k − fcr,k + fsh,k =

−133.4 × 10−6 N

+0.799 × 10−6 Nmm

With εr,k = −133.4 × 10−6 and κk = +0.799 × 10−6 mm−1 , the ﬁnal strain at the top of the slab (y = −450 mm) and at the bottom of the steel I-section (y = 300 mm) at time τk are: εk(top) = εr,k + (−450) × κk = −493.2 × 10−6 εk(btm) = εr,k + 300 × κk = +106.5 × 10−6 The ﬁnal concrete stresses at the top and bottom of the slab at time τk are (Eq. 5.41a): σc,k(top) = 9524

! −133.4 × 10−6 1 −450 − (−600 × 10−6 ) 0.799 × 10−6

= +1.02 MPa

! −133.4 × 10−6 −6 σc,k(btm) = 9524 1 −300 − (−600 × 10 ) 0.799 × 10−6 = +2.16 MPa and the ﬁnal stress in the steel reinforcement is (Eq. 5.41b): σs(1),k = 200,000 [−133.4 − 375 × 0.799] × 10−6 = −86.6 MPa The ﬁnal stresses at the top and bottom ﬁbres of the steel I-beam are (Eq. 5.65): σss,k(top) = 200,000 [−133.4 − 300 × 0.799] × 10−6 = −74.6 MPa σss,k(btm) = 200,000 [−133.4 + 300 × 0.799] × 10−6 = +21.3 MPa

Uncracked sections 189 The ﬁnal stress and strain distributions are illustrated in Fig 5.18. The shrinkageinduced ﬁnal curvature (+0.799 × 10−6 mm−1 ) is almost 70 per cent of the change in curvature with time in Example 5.7 (where κ = κk − κ0 = 1.142 × 10−6 mm−1 ). In addition, the tensile stress induced in the bottom ﬁbre of the concrete due to the restraint to shrinkage may be sufﬁcient to cause cracking in the concrete. −493.2

1.02

−86.6

2.16

−74.6 e

x

y (a) Cross-section

s

106.5 (b) Strain diagram (× 10−6)

21.3 (c) Stress diagram (MPa)

Figure 5.18 Shrinkage-induced stress and strain distributions at τk for Example 5.8.

5.7 Composite concrete-concrete cross-sections The analysis of a cross-section consisting of different reinforced or prestressed concrete elements acting compositely together and subjected to a sustained bending moment and axial force is presented here. A typical cross-section is shown in Fig 5.19. This particular cross-section is made up of two concrete elements, a precast pretensioned I-section (Element 1) and an in-situ slab deck (Element 2). Each concrete element may have different creep and shrinkage characteristics, as well as different elastic moduli. In the subsequent analyses, perfect bond is assumed between each concrete element, as well as between the concrete and the bonded steel reinforcement.

ds(1) As(1) ds(3) ds(2)

As(3)

dref ds(4)

dp(2)

dc(2)

As(2)

dp(1)

x

Centroidal axis of precast concrete girder (Element 1), Ac(1)

dc(1)

Centroidal axis of in-situ concrete deck (Element 2), Ac(2)

Ap(1) Ap(2) As(4) y

Figure 5.19 Typical concrete-concrete composite section.

190 Uncracked sections The general procedure introduced in Sections 5.3–5.5 for reinforced and prestressed concrete cross-sections is readily extended to include composite sections comprising two or more concrete components. Consider a composite section formed with mc different concrete components. For the i-th concrete component (with i = 1, . . . , mc ), the area is Ac(i) , and the ﬁrst and second moments of the area about the reference axis are Bc(i) and Ic(i) , respectively. For clarity and completeness, the short-term analysis (assuming linear-elastic material behaviour) and the time-dependent analyses using both the AEMM and the SSM are presented separately in the following. 5.7.1 Short-term analysis As outlined in Section 5.3, the constitutive relationships for each material for use in the instantaneous analysis are (Eq. 5.4): σc(i),0 = Ec(i),0 ε0

(5.67a)

σs(i),0 = Es(i) ε0 σp(i),0 = Ep(i) ε0 + εp(i),init

(5.67b) (5.67c)

Similar to Eq. 5.7a, the internal actions carried by the i-th concrete element (for inclusion in the equilibrium equations) can be expressed as: Nc(i),0 =

Ac(i)

σc(i),0 dA =

Ac(i)

Ec(i),0 εr,0 + yκ0 dA

= Ac(i) Ec(i),0 εr,0 + Bc(i) Ec(i),0 κ0 Mc(i),0 = yσc(i),0 dA = Ec(i),0 y εr,0 + yκ0 dA Ac(i)

(5.68a)

Ac(i)

= Bc(i) Ec(i),0 εr,0 + Ic(i) Ec(i),0 κ0

(5.68b)

and, as in Eq. 5.12, the governing system of equilibrium equations is: re,0 = D0 ε0 + fp,init

(5.69)

Solving for the unknown strain variables gives (Eq. 5.14): ε0 = D−1 re,0 − fp,init = F0 re,0 − fp,init 0

(5.70)

where D0 = F0 =

RA,0 RB,0 RB,0 RI,0 1 RA,0 RI,0 − R2B0

(5.71a)

RI,0 −RB,0 −RB,0 RA,0

(5.71b)

Uncracked sections 191

εr,0 ε0 = κ0

Ne,0 re,0 = Me,0 mp Ap(i) Ep(i) εp(i),init fp,init = yp(i) Ap(i) Ep(i) εp(i),init i=1

(5.71c) (5.71d)

(5.71e)

The cross-sectional rigidities forming the D0 matrix in Eq. 5.71a are: RA,0 =

mc

Ac(i) Ec(i),0 +

ms

i=1

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ec(i),0 + RA,s + RA,p

i=1

(5.72a) RB,0 =

mc

Bc(i) Ec(i),0 +

i=1

=

ms

ys(i) As(i) Es(i) +

i=1

mc

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ec(i),0 + RB,s + RB,p

(5.72b)

i=1

RI,0 =

mc

Ic(i) Ec(i),0 +

i=1

=

ms

2 ys(i) As(i) Es(i) +

i=1

mc

Ic(i) Ec(i),0 + RI,s + RI,p

mp

2 yp(i) Ap(i) Ep(i)

i=1

(5.72c)

i=1

where for convenience the following notation is introduced for the rigidities of the reinforcement and tendons: ms As(i) Es(i) (5.73a) RA,s = i=1

RB,s =

ms

ys(i) As(i) Es(i)

(5.73b)

2 ys(i) As(i) Es(i)

(5.73c)

i=1

RI,s =

ms i=1 mp

RA,p =

Ap(i) Ep(i)

(5.74a)

yp(i) Ap(i) Ep(i)

(5.74b)

2 yp(i) As(i) Ep(i)

(5.74c)

i=1

RB,p =

mp i=1

RI,p =

mp i=1

192 Uncracked sections The stress distribution is calculated from Eq. 5.16: σc(i),0 = Ec(i),0 ε0 = Ec(i),0 [1

y]ε0

σs(i),0 = Es(i) ε0 = Es(i) [1 ys(i) ]ε0 σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) [1

(5.75a) (5.75b) yp(i) ]ε0 + Ep(i) εp(i),init

(5.75c)

where ε0 = εr,0 + yκ0 = [1 y]ε0 . 5.7.2 Time analysis – AEMM For the analysis of stresses and deformations on a composite concrete-concrete crosssection at time τk after a period of sustained loading, the AEMM may be used, as outlined in Section 5.4. The stress–strain relationships for each concrete element and for each layer of reinforcement and tendons at τk are as follows (Eq. 5.22): σc(i),k = Fe(i),0 σc(i),0 Ee(i),k εk − εsh(i),k + σs(i),k = Es(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(5.76a) (5.76b) (5.76c)

In this case the contribution of the i-th concrete component to the internal axial force and moment can be determined as (similar to Eq. 5.27): Nc(i),k =

Ac(i)

σc(i),k dA =

Ac(i)

Ee(i),k εr,k + yκk − εsh(i),k + Fe(i),0 σc(i),0 dA

= Ac(i) Ee(i),k εr,k + Bc(i) Ee(i),k κk − Ac(i) Ee(i),k εsh(i),k + Fe(i),0 Nc(i),0 (5.77a) Mc(i),k = yσc(i),k dA = y Ee(i),k εr,k + yκk − εsh(i),k + Fe(i),0 σc(i),0 dA Ac(i)

Ac(i)

= Bc(i) Ee(i),k εr,k + Ic(i) Ee(i),k κk − Bc(i) Ee(i),k εsh(i),k + Fe(i),0 Mc(i),0

(5.77b)

The equilibrium equations are (Eq. 5.34): re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k

(5.78)

and solving gives the strain at time τk (Eq. 5.39): εk = D−1 re,k − fcr,k + fsh,k − fp,init + fp.rel,k k = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(5.79)

Uncracked sections 193 where

ε εk = r,k κk

Ne,k re,k = Me,k

RA,k RB,k Dk = RB,k RI,k Fk =

1

(5.80a) (5.80b) (5.80c)

RI,k

−RB,k

RA,k RI,k − R2B,k −RB,k

(5.80d)

RA,k

and the cross-sectional rigidities at τk are:

RA,k =

mc

Ac(i) Ee(i),k +

i=1

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ee(i),k + RA,s + RA,p

i=1

(5.81a) RB,k =

mc

Bc(i) Ee(i),k +

i=1

=

mc

ms

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ee(i),k + RB,s + RB,p

(5.81b)

i=1

RI,k =

mc

Ee(i),k + Ic(i)

i=1

=

mc

ms

2 ys(i) As(i) Es(i) +

mp

2 yp(i) Ap(i) Ep(i)

i=1

i=1

Ee(i),k + RI,s + RI,p Ic(i)

(5.81c)

i=1

In Eq. 5.78, the effects of creep and shrinkage of the concrete elements are included by (see Eqs 5.36 and 5.37):

fcr,k =

mc

Fe(i),0

i=1

fsh,k =

mc Ac(i) i=1

Bc(i)

Nc(i),0 Mc(i),0

=

mc i=1

Ee(i),k εsh(i),k

Fe(i),0 Ec(i),0

Ac(i) εr,0 + Bc(i) κ0 Bc(i) εr,0 + Ic(i) κ0

(5.82)

(5.83)

194 Uncracked sections The initial strain in the prestressing steel and relaxation are accounted for using (Eq. 5.38): fp,init =

mp i=1

fp.rel,k =

mp

Ap(i) Ep(i) εp(i),init

yp(i) Ap(i) Ep(i) εp(i),init

i=1

Ap(i) Ep(i) εp(i),init ϕp (τk , σp(i),init ) yp(i) Ap(i) Ep(i) εp(i),init ϕp (τk , σp(i),init )

(5.84a)

(5.84b)

The stress distributions at time τk in each concrete element and in the reinforcement and tendons are (Eq. 5.41): Fe(i),0 σc(i),0 Ee(i),k εk − εsh(i),k + σc(i),k = & ' = Ee(i),k 1 y εk − εsh(i),k + Fe(i),0 σc(i),0 σs(i),k = Es(i) εk = Es(i) 1 ys(i) εk σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(5.85a) (5.85b)

(5.85c)

where εk = εr,k + yκk = 1 y εk .

Example 5.9 The composite cross-section shown in Fig. 5.20 forms part of a bridge deck and consists of an in-situ reinforced concrete deck and a precast post-tensioned I-section (with bonded tendons). At time τ0 with both concrete elements acting compositely, the road surface and other superimposed dead load are placed on the bridge, thereby introducing an increment of external moment Me = 400 kNm at the section shown. Both the immediate and ﬁnal long-term changes of stress caused by Me are to be calculated. For the precast I-girder: Ec(1) (τ0 ) = 32,000 MPa; ϕ(1) (∞, τ0 ) = 2.0; χ(1) (∞, τ0 ) = 0.65. For the concrete deck: Ec(2) (τ0 ) = 25,000 MPa; ϕ(2) (∞, τ0 ) = 2.5; χ(2) (∞, τ0 ) = 0.65. For the steel reinforcement and tendons: Es = Ep = 200,000 MPa. In this example, only the increments of stress and strain caused by Me are to be calculated. In the actual bridge girder, these must be added to the increments of stress and strain caused by the prestress, self-weight, live load, shrinkage of the concrete, relaxation of the prestressing steel and, if applicable, temperature changes.

Uncracked sections 195 As(1) = 2700 mm2 2400

75 210 1030 1160 1240

x 150

As(2) = 900 mm2 752 Centroidal axis of precast concrete I-girder Ac(1) = 317 × 103 mm2 Ic(1) = 49,900 × 106 mm4

Centroidal axis of in-situ concrete slab

1300

Ap(1) = 800 mm2 Ap(2) = 800 mm2 As(3) = 1800 mm2 y

Figure 5.20 Details of the cross-section for Example 5.9.

In the following solution, the top surface of the in-situ slab is selected as the reference axis, as shown in Fig. 5.20, (i.e. dref = 0 mm) and its distances from the steel layers are: ys(1) = 75 mm, ys(2) = 210 mm, ys(3) = 1240 mm, yp(1) = 1030 mm and yp(2) = 1160 mm. The applied loads are:

0N re,0 = 400 × 106 Nmm As no prestressing forces and shrinkage effects are considered in this problem, the vectors f p,init , f p.rel,0 , f p.rel,k and f sh,k are all nil:

0N fp,init = 0 Nmm

0N fp.rel,0 = fp.rel,k = 0 Nmm

0N fsh,k = 0 Nmm

Short-term analysis (at time τ0 ) The geometric properties of the precast girder cross-section are calculated as: Ac(1) = Agross − As(2) − As(3) − Ap(1) − Ap(2) = 312,700 mm2 Bc(1) = Agross dc(1) − dref − As(2) ys(2) + As(3) ys(3) − Ap(1) yp(1) + Ap(2) yp(2) = 234.2 × 106 mm3 2 2 2 Ic(1) = Igross + Agross dc(1) − dref − As(2) ys(2) + As(3) ys(3) 2 2 − Ap(1) yp(1) + Ap(2) yp(2) = 224.4 × 109 mm4

196 Uncracked sections and those of the concrete deck are: Ac(2) = bD − As(1) = 357,300 mm2 Bc(2) = bD(D/2 − dref ) − As(1) ys(1) = 26.79 × 106 mm3

2 bD3 D 2 Ic(2) = + bD − dref − As(1) ys(1) = 2684 × 106 mm4 12 2 The instantaneous cross-sectional rigidities are (Eq. 5.72): RA,0 = Ac(1) Ec(1),0 + Ac(2) Ec(2),0 + As(1) + As(2) + As(3) Es + Ap(1) + Ap(2) Ep = 20,340 × 106 N RB,0 = Bc(1) Ec(1),0 + Bc(2) Ec(2),0 + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 9039 × 109 Nmm 2 2 2 RI,0 = Ic(1) Ec(1),0 + Ic(2) Ec(2),0 + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 8198 × 1012 Nmm2 The matrix F0 can then be determined as (Eq. 5.71b): F0 =

1

RI,0 −RB,0 −RB,0 RA,0

RA,0 RI,0 − R2B,0 −106.3 × 10−15 N−1 mm−1 96.42 × 10−12 N−1 = −106.3 × 10−15 N−1 mm−1 239.2 × 10−18 N−1 mm−2

The strain vector ε0 containing the unknown strain variables is determined from Eq. 5.70:

96.42 × 10−12 −106.3 × 10−15 −106.3 × 10−15 239.2 × 10−18 ( ) 0 0 −42.5 × 10−6 × − = 0 400 × 106 0.095 × 10−6 mm−1

ε0 = F0 re,0 − fp,init =

The increment of strain at the reference axis and the increment of curvature caused by the imposed moment Me = 400 kNm are therefore εr,0 = −42.5×10−6 and κ0 = 0.095×10−6 mm−1 and, from Eq. 5.1, the increments of top (y = 0 mm) and bottom (y = 1300 mm) ﬁbre strains are: ε0(top) = εr,0 + 0 × κ0 = −42.5 × 10−6 and ε0(btm) = εr,0 + 1300 × κ = 81.8 × 10−6

Uncracked sections 197 From Eq. 5.75a, the changes in the top and bottom ﬁbre stresses on the precast I-section are: σc(1),0(top) = Ec(1),0 εc(1),0(top) = 32,000 × (−42.5 + 150 × 0.095) × 10−6 = −0.90 MPa σc(1),0(btm) = Ec(1),0 εc(1),0(btm) = 32,000 × (−42.5 + 1300 × 0.095) × 10−6 = +2.62 MPa and on the concrete deck: σc(2),0(top) = Ec(2),0 εc(2),0(top) = 25,000 × (−42.5 + 0 × 0.095) × 10−6 = −1.06 MPa σc(2),0(btm) = Ec(2),0 εc(2),0(btm) = 25,000 × (−42.5 + 150 × 0.095) × 10−6 = −0.70 MPa The increments of stress in the non-prestressed reinforcement are obtained from Eq. 5.75b as: −42.5 × 10−6 3 σs(1),0 = 200 × 10 × 1 75 = −7.1 MPa 0.095 × 10−6 −6 −42.5 × 10 σs(2),0 = 200 × 103 × 1 210 = −4.5 MPa 0.095 × 10−6 −42.5 × 10−6 3 σs(3),0 = 200 × 10 1 1240 = 15.2 MPa 0.095 × 10−6 and in the prestressing steel (Eq. 5.75c)

σp(1),0 = Ep 1 yp(1)

−42.5 × 10−6 ε0 = 200 × 10 × 1 1030 0.095 × 10−6

−42.5 × 10−6 ε0 = 200 × 10 × 1 1160 0.095 × 10−6

= 11.2 MPa

σp(2),0 = Ep 1 yp(2)

3

3

= 13.7 MPa

Long-term analysis (at time τk = ∞) For the long-term analysis at time τk the age-adjusted material properties for the two concrete elements are obtained from Eqs 4.35 and 4.46: Ee(1),k =

Ec(1),0 32,000 = 13,910 MPa = 1 + χ(1) (τk , τ0 ) ϕ(1) (τk , τ0 ) 1 + 0.65 × 2.0

198 Uncracked sections Ec(2),0 25,000 = 9523 MPa = 1 + χ(2) (τk , τ0 ) ϕ(2) (τk , τ0 ) 1 + 0.65 × 2.5 ϕ(1) (τk , τ0 ) χ(1) (τk , τ0 ) − 1 2.0 × (0.65 − 1) Fe(1),0 = = −0.304 = 1 + χ(1) (τk , τ0 ) ϕ(1) (τk , τ0 ) 1 + 0.65 × 2.0 ϕ(2) (τk , τ0 ) χ(2) (τk , τ0 ) − 1 2.5 × (0.65 − 1) Fe(2),0 = = −0.333 = 1 + 0.65 × 2.5 1 + χ(2) (τk , τ0 ) ϕ(2) (τk , τ0 ) Ee(2),k =

Creep effects are accounted for using Eq. 5.82:

Ac(1) εr,0 + Bc(1) κ0 Ac(2) εr,0 + Bc(2) κ0 fcr,k = Fe(1),0 Ec(1),0 + Fe(2),0 Ec(2),0 Bc(1) εr,0 + Ic(1) κ0 Bc(2) εr,0 + Ic(2) κ0 16.5 × 103 N = −104.8 × 106 Nmm The cross-sectional rigidities at time τk are calculated from Eq. 5.81: RA,k = Ac(1) Ee(1),k + Ac(2) Ee(2),k + As(1) + As(2) + As(3) Es + Ap(1) + Ap(2) Ep = 9153 × 106 N RB,k = Bc(1) Ee(1),k + Bc(2) Ee(2),k + As(1) ys(1) + As(2) ys(2) + As(3) ys(3) Es + Ap(1) yp(1) + Ap(2) yp(2) Ep = 4389 × 109 Nmm 2 2 2 RI,k = Ic(1) Ee(1),k + Ic(2) Ee(2),k + As(1) ys(1) Es + As(2) ys(2) + As(3) ys(3) 2 2 + Ap(1) yp(1) + Ap(2) yp(2) Ep = 4097 × 1012 Nmm2 Matrix Fk is then determined as (Eq. 5.80d): −240.5 × 10−15 N−1 mm−1 224.6 × 10−12 N−1 Fk = −240.5 × 10−15 N−1 mm−1 501.7 × 10−18 N−1 mm−2 The strain vector εk at time τk caused by the sustained moment Me is obtained from Eq. 5.79: −125.1 × 10−6 N εk = Fk re,k − fcr,k = 0.257 × 10−6 Nmm The ﬁnal increments of strains at the top and bottom ﬁbres of the cross-section are (Eq. 5.1): εk(top) = εr,k + 0 × κk = −125.1 × 10−6 εk(btm) = εr,k + 1300 × κk = 209.2 × 10−6

Uncracked sections 199 The increments of stress at time τk in the top and bottom ﬁbres of the precast I-section are determined using Eq. 5.85a: σc(1),k(top) = Fe(1),0 σc(1),0(top) Ee(1),k εc(1),k(top) − εsh(1),k + = 13,913 × (−125.1 + 150 × 0.257) × 10−6 − 0.304 × (−0.90) = −0.93 MPa and Ee(1),k εc(1),k(btm) − εsh(1),k + Fe(1),0 σc(1),0(btm) = 2.11 MPa σc(1),k(btm) = Similarly, for the concrete deck: σc(2),k(top) = Ee(2),k εc(2),k(top) − εsh(2),k + Fe(2),0 σc(2),0(top) = 9523 × (−125.1 + 0 × 0.257) × 10−6 − 0.333 × (−1.06) = −0.84 MPa Fe(2),0 σc(2),0(btm) = −0.59 MPa Ee(2),k εc(2),k(btm) − εsh(2),k + σc(2),k(btm) = The ﬁnal increments of stress in the non-prestressed reinforcement are obtained from Eq. 5.85b: −125.1 × 10−6 σs(1),k = 200 × 10 × 1 75 = −21.2 MPa 0.257 × 10−6 −125.1 × 10−6 3 σs(2),k = 200 × 10 × 1 210 = −14.2 MPa 0.257 × 10−6 −125.1 × 10−6 3 σs(3),k = 200 × 10 1 1240 = +38.8 MPa 0.257 × 10−6 3

and for the prestressing steel, Eq. 5.85c gives: σp(1),k = Ep 1 yp(1) εk + Ep εpinit(1) −6 −125.1 × 10 + 0 = 27.9 MPa = 200 × 103 × 1 1030 0.257 × 10−6 and σp(2),k = Ep 1 yp(2) εk + Ep εpinit(2) −6 −125.1 × 10 = 200 × 103 × 1 1160 + 0 = 34.6 MPa 0.257 × 10−6

200 Uncracked sections The stress and strain distributions at times τ0 and at τk are shown in Fig. 5.21.

x

−125.1 −42.5

−1.06 −0.84 s −7.1 −21.2 −0.93−0.90 −4.5 −0.70 −0.59 −14.2

e

Time, t0 Time, tk 11.2 13.7 15.2

y (a) Cross-section

81.8 209.2 (b) Strain diagram (× 10−6)

27.9 34.6 38.8 2.11 2.62 (c) Stress diagram (MPa)

Figure 5.21 Strain and stress distributions for Example 5.9.

5.7.3 Time analysis – SSM The SSM outlined in Section 5.5 is extended in the following to analyse a composite cross-section with mc different concrete elements. Similar to Eqs 4.25 and 5.44, the constitutive relationships for the different materials at time τj are: j−1

σc(i),j = Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n

(5.86a)

n=0

σs(i),j = Es(i) εj − εs(i),set−1 σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j − εp(i),set−1

(5.86b) (5.86c)

where the additional strain terms εc(i),set−1 , εs(i),set−1 , εp(i),set−1 have been included to account for variations in the cross-section when different parts of the cross-section are cast at different times, such as occurs, for example, in sequential casting. The term set refers to the time step at which a particular concrete element sets and begins to contribute to the structural stiffness. The inclusion of the strains εc(i),set−1 , εs(i),set−1 , εp(i),set−1 in Eq. 5.86 ensures that all new components are initially unloaded. Similar treatment can be given to the grouting of post-tensioning ducts at some time after the transfer of prestress, as illustrated subsequently in Example 5.10. In the formulation adopted here (and illustrated in Example 5.10), two steps are considered in the solution whenever a new concrete element is added to the crosssection. The ﬁrst step involves the calculation of the cross-sectional response just before the element sets, at τset−1 , and the second step involves the calculation of the response just after the element starts to contribute to the structural stiffness, at τset . Obviously, for situations not related to sequential casting, i.e. where all concrete elements are in place from the beginning of the analysis, the terms εc(i),set−1 , εs(i),set−1 and εp(i),set−1 in Eq. 5.86 are all set to zero.

Uncracked sections 201 Similarly to Eq. 5.48, the axial force and moment resisted by the i-th concrete element are: ⎡ ⎤ j−1 ⎣Ec(i),j εj − εsh(i),j − εc(i),set−1 + Nc(i),j = σc(i),j dA = Fe(i),j,n σc(i),n⎦ dA Ac(i)

Ac(i)

n=0

= Ac(i) Ec(i),j εr,j − εr,set−1 + Bc(i) Ec(i),j κj − κset−1 − Ac(i) Ec(i),j εsh(i),j +

j−1

Fe(i),j,n Nc(i),n

n=0

Mc(i),j =

yσc(i),j dA =

Ac(i)

(5.87a) ⎡

⎤ j−1 y ⎣Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n⎦ dA

Ac(i)

n=0

= Bc(i) Ec(i),j εr,j − εr,set−1 + Ic(i) Ec(i),j κj − κset−1 − Bc(i) Ec(i),j εsh(i),j +

j−1

Fe(i),j,n Mc(i),n

(5.87b)

n=0

in which εr,set−1 and κset−1 deﬁne the strain diagram immediately before the i-th concrete element sets at τset−1 . As for the earlier analyses (Eq. 5.54), the governing equilibrium equations are: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j − fset,j

(5.88)

and solving for the unknown strain distribution at τj gives: re,j − fcr,j + fsh,j − fp,init + fp.rel,j + fset,j εj = D−1 j = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j + fset,j

(5.89)

where (as before):

εr,j κj

RA,j RB,j Dj = RB,j RI,j

Ne,j re,j = Me,j εj =

Fj =

fp,init =

1

(5.90a) (5.90b) (5.90c)

RI,j −RB,j −RB,j RA,j

RA,j RI,j − R2B,j mp Ap(i) Ep(i) εp(i),init i=1

yp(i) Ap(i) Ep(i) εp(i),init

(5.90d)

(5.90e)

202 Uncracked sections mp Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) fp.rel,j = yp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) i=1 fcr,j =

j−1 mc

(5.90f)

Fe(i),j,n rc(i),n

(5.90g)

i=1 n=0

fsh,j =

mc Ac(i) i=1

Bc(i)

Ec(i),j εsh(i),j

(5.90h)

while f set.j is deﬁned as:

fset,j =

mc

fc(i).set,j +

i=1

ms

fs(i).set,j +

i=1

mp

fp(i).set,j

(5.90i)

i=1

and fc(i).set,j = fs(i).set,j =

Ac(i) Ec(i),j εr,set−1 + Bc(i) Ec(i),j κset−1

(5.90j)

Bc(i) Ec(i),j εr,set−1 + Ic(i) Ec(i),j κset−1 As(i) Es(i) εr,set−1 + Bs(i) Es(i) κset−1

fp(i).set,j =

Bs(i) Es(i) εr,set−1 + Is(i) Es(i) κset−1 Ap(i) Ep(i) εr,set−1 + Bp(i) Ep(i) κset−1

(5.90k)

(5.90l)

Bp(i) Ep(i) εr,set−1 + Ip(i) Ep(i) κset−1

The i-th component of the cross-section is included in the calculation of f set,j only when the instant in time τj is greater than or equal to τset of the i-th component. The axial force and moment resisted by the concrete at any time τi (required in Eq. 5.90g) is determined as: rc(i),n =

Nc(i),n

Mc(i),n

= Dc(i),n (εn − εset−1 ) +

n−1

Fe(i),n,l rc(i),l −

l=0

Ac(i) Bc(i)

Ec(i),n εsh(i),n (5.91)

where εset−1 is the vector containing εr,set−1 and κset−1 and: Ac(i) Bc(i) Ec(i),n Dc(i),n = Bc(i) Ic(i)

(5.92)

The term Dc(i),n in Eq. 5.91 includes the properties of the i-th concrete element introduced at τset while εset−1 deﬁnes the strain diagram at time τset−1 , i.e. immediately prior to the setting of the concrete in the i-th element.

Uncracked sections 203 The cross-sectional rigidities to be used at τj are: RA,j =

mc

Ac(i) Ec(i),j +

i=1

ms

As(i) Es(i) +

i=1

mp

Ap(i) Ep(i) =

i=1

mc

Ac(i) Ec(i),j + RA,s + RA,p

i=1

(5.93a) RB,j =

mc

Bc(i) Ec(i),j +

i=1

=

mc

ms

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i)

i=1

Bc(i) Ec(i),j + RB,s + RB,p

(5.93b)

i=1

RI,j =

mc

Ic(i) Ec(i),j +

i=1

=

mc

ms

2 ys(i) As(i) Es(i) +

i=1

mp

2 yp(i) Ap(i) Ep(i)

i=1

Ic(i) Ec(i),j + RI,s + RI,p

(5.93c)

i=1

and ﬁnally, the stress distributions at τj can be determined from j−1

σc(i),j = Ec(i),j εj − εsh(i),j − εc(i),set−1 + Fe(i),j,n σc(i),n n=0 j−1

= Ec(i),j

& ' 1 y εj − εset−1 − εsh(i),j + Fe(i),j,n σc(i),n

(5.94a)

n=0

σs(i),j = Es(i) εj − εs(i),set−1 = Es(i) 1 ys(i) εj − εset−1 σp(i),j = Ep(i) εj + εp(i),init − εp.rel(i),j − εp(i),set−1 = Ep(i) 1 yp(i) εj − εset−1 + Ep(i) εp(i),init − Ep(i) εp.rel(i),j

(5.94b)

(5.94c)

where εj = εr,j + yκj = 1 y εj .

Example 5.10 The bridge girder with cross-section shown in Fig. 5.20 is subjected to the following load history. The I-section is cast and moist cured for 7 days. At age 7 days, the member is post-tensioned with an initial prestressing force of 2000 kN (Pp,init = 1000 kN in each tendon). The diameter of each prestressing duct is 60 mm. The moment at the cross-section due to the self-weight of the girder is M7 = 550 kNm and is ﬁrst applied to the cross-section during the posttensioning operation at age 7 days. Shrinkage of the concrete in the I-girder also begins to develop at this time. At age 40 days, the slab deck is cast and cured

204 Uncracked sections and the moment caused by the weight of the wet concrete, M40 = 620 kNm, is ﬁrst applied to the precast I-section. The post-tensioning ducts are also grouted at this time (i.e. at age 40 days). Composite action gradually begins to develop as soon as the concrete in the deck sets and the grout within the ducts hardens. Full composite action may not be achieved for several days. However, it is here assumed that the deck and the I-section act compositely and that the prestressing tendons are bonded to the concrete at all times after age 40 days. Shrinkage of the deck is assumed to also begin at age 40 days. At τ = 60 days, the road surface is placed and other superimposed dead loads are applied to the bridge, thereby introducing an additional moment of M60 = 400 kNm. Thereafter, the loads are assumed to remain constant in time. The stress and strain distributions on the cross-section are to be calculated at the following times: (i) immediately after the application of the prestress at age 7 days; (ii) before and after the slab deck is cast at age 40 days; (iii) after the deck and I-section act compositely at age 40 days; (iv) before and after the road surface is placed at age 60 days; (v) at age 30,000 days (i.e. about 80 years) assuming the applied actions acting at age 60 days remain constant thereafter. Based on this loading history the following steps 0 to 6 are considered in the worked example: Step

Age (in days)

0

7

1

40 −

2

40 +

3

40 ++

4

60 −

5

60 +

6

30,000

Description of event Prestressing force applied to the section. Application of M7 = 550 kNm (short-term analysis). Time step introduced to determine the effects of creep, shrinkage and relaxation in the I-girder from age 7 days to age 40 days under the action introduced at 7 days and held constant thereafter (time analysis). The deck is poured introducing an additional moment of M40 = 620 kNm to be resisted by the I-section alone (short-term analysis) Change in cross-section due to grouting of ducts and deck acting compositely with the I-section (from this point in time). Time step introduced to evaluate the time-dependent behaviour of the composite section under constant actions between ages 40 and 60 days (time analysis). Road surface added causing an additional moment of M60 = 400 kNm to be applied to the composite section (short-term analysis). Time step introduced to evaluate the ﬁnal long-term behaviour assuming loads remain constant after age 60 days.

Uncracked sections 205 The material properties are: For all reinforcing steel and tendons: Es = Ep = 200 GPa ϕp (7, σp,init ) = 0 ϕp (40, σp,init ) = 0.015 ϕp (60, σp,init ) = 0.02 ϕp (30,000, σp,init ) = 0.03 For the precast I-section (Concrete element 1): Ec(1),0 = 25 GPa Ec(1),1 = Ec(1),2 = Ec(1),3 = 32 GPa Ec(1),4 = Ec(1),5 = 34 GPa Ec(1),6 = 38 GPa ϕ(1) (7, 7) = 0 ϕ(1) (40, 7) = 0.8 ϕ(1) (60, 7) = 1.0 ϕ(1) (30,000, 7) = 2.5 ϕ(1) (40, 40) = 0 ϕ(1) (60, 40) = 0.8 ϕ(1) (30,000, 40) = 1.8 ϕ(1) (60, 60) = 0 ϕ(1) (30,000, 60) = 1.6 εsh(1) (7) = 0 εsh(1) (40) = −100 × 10−6 εsh(1) (60) = −150 × 10−6 εsh(1) (30,000) = −400 × 10−6 For the concrete deck (Concrete element 2): Ec(2),3 = 18 GPa Ec(2),4 = Ec(2),5 = 25 GPa Ec(2),6 = 30 GPa

206 Uncracked sections ϕ(2) (40, 40) = 0 ϕ(2) (60, 40) = 2.0 ϕ(2) (30,000, 40) = 3.5 ϕ(2) (60, 60) = 0 ϕ(2) (30,000, 60) = 2.8 εsh(2) (40) = 0 εsh(2) (60) = −200 × 10−6 εsh(1) (30,000) = −600 × 10−6 As for Example 5.9, the top ﬁbre of the concrete deck is selected as the reference axis, i.e. dref = 0 mm, and the distances of the steel and prestressing layers from the reference axis are ys(1) = 75 mm, ys(2) = 210 mm, ys(3) = 1240 mm, yp(1) = 1030 mm and yp(2) = 1160 mm. The external loads applied at each step are: 0N re,0 = re,1 = 550 × 106 Nmm

0N re,2 = re,3 = re,4 = 1170 × 106 Nmm

0N re,5 = re,6 = 1570 × 106 Nmm

The concrete material coefﬁcients to be used in the various analyses are as follows: For the precast I-section (Element 1): Jc(1) (7, 7) = 4 × 10−5 MPa−1 Jc(1) (40, 7) = 7.2 × 10−5 MPa−1 Jc(1) (60, 7) = 8 × 10−5 MPa−1 Jc(1) (30,000, 7) = 14 × 10−5 MPa−1 Jc(1) (40, 40) = 3.125 × 10−5 MPa−1 Jc(1) (60, 40) = 5.625 × 10−5 MPa−1 Jc(1) (30,000, 40) = 8.75 × 10−5 MPa−1 Jc(1) (60, 60) = 2.941 × 10−5 MPa−1 Jc(1) (30,000, 60) = 7.647 × 10−5 MPa−1

Uncracked sections 207 Jc(1) (30,000, 30,000) = 2.631 × 10−5 MPa−1 Fe(1),1,0 = Fe(1),2,0 = Fe(1),3,0 = −1.304 Fe(1),4,0 = Fe(1),5,0 = −0.807 Fe(1),6,0 = −1.995 Fe(1),4,3 = Fe(1),5,3 = −0.912 Fe(1),6,3 = −0.419 Fe(1),6,5 = −1.906 Fe(1),i,j = 0 if τi = τj εsh(1) (7) = 0 εsh(1) (40) = εsh(1),1 = εsh(1),2 = εsh(1),3 = −100 × 10−6 εsh(1) (60) = εsh(1),4 = εsh(1),5 = −150 × 10−6 εsh(1) (30,000) = εsh(1),6 = −400 × 10−6 For the concrete deck (Element 2): Jc(2) (40, 40) = 5.555 × 10−5 MPa−1 Jc(2) (60, 40) = 16.66 × 10−5 MPa−1 Jc(2) (30,000, 40) = 25 × 10−5 MPa−1 Jc(2) (60, 60) = 4.0 × 10−5 MPa−1 Jc(2) (30,000, 60) = 15.2 × 10−5 MPa−1 Jc(2) (30,000, 30,000) = 3.333 × 10−5 MPa−1 Fe(2),4,3 = Fe(2),5,3 = −3.166 Fe(2),6,3 = −2.94 Fe(2),6,5 = −3.56 Fe(2),i,j = 0 if τi = τj εsh(2) (40) = εsh(2),1 = εsh(2),2 = εsh(2),3 = 0 εsh(2) (60) = εsh(2),4 = εsh(2),5 = −200 × 10−6 εsh(2) (30,000) = εsh(2),6 = −600 × 10−6 The initial prestress is included in the analysis using: 2000 × 103 N fp,init = 2190 × 106 Nmm

208 Uncracked sections The concrete area of the I-section contributing to the cross-sectional rigidity changes when the prestressing ducts are grouted. For clarity, the concrete properties of the I-section before grouting are referred to as Ac(1a) , Bc(1a) and Ic(1a) , and after grouting as Ac(1b) , Bc(1b) and Ic(1b) . The procedures required to analyse the I-section in the ﬁrst three steps (before the concrete deck is cast) are identical to those illustrated in Examples 5.2 and 5.6 and, for this reason, only the results of the analyses for Steps 1, 2 and 3 are presented here.

Step 0: Short-term analysis at age τ = 7 days Concrete properties: Ac(1a) = 308.6 × 103 mm2 ; Bc(1a) = 229.7 × 106 mm3 ; and Ic(1a) = 219.5 × 109 mm4 . Cross-sectional rigidities: RA,0 = 8256 × 106 N; RB,0 = 6228 × 109 Nmm; and RI,0 = 6050 × 1012 Nmm2 . The matrix F0 : F0 =

542.2 × 10−12 N−1

−558.2 × 10−15 N−1 mm−1

−558.2 × 10−15 N−1 mm−1

739.9 × 10−18 N−1 mm−2

Strain at reference axis and curvature: εr,0 = −169.0 × 10−6 and κ0 = −0.097 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε0(top) = −183.6 × 10−6 and ε0(btm) = −295.2 × 10−6 . Concrete stresses: σc(1),0(top) = −4.60 MPa and σc(1),0(btm) = −7.38 MPa. Reinforcement stresses: σs(2),0 = −37.9 MPa and σs(3),0 = −57.9 MPa. Stresses in tendons: σp(1),0 = 1250 MPa and σp(2),0 = 1250 MPa. The concrete stress resultants at τ0 = 7 days are: −1862 × 103 N . rc(1),0 = −1504 × 106 Nmm

Step 1: Time analysis – SSM at age τ1 = 40 days Creep and shrinkage of the concrete as well as relaxation of the prestressing steel in the I-section are accounted for with: fcr,1 =

2427 × 103 N

1961 × 106 Nmm

fsh,1 =

−987.7 × 103 N

−735.3 × 106 Nmm

fp.rel,1 =

30 × 103 N

32.85 × 106 Nmm

Uncracked sections 209 Cross-sectional rigidities: RA,1 = 10416 × 106 N; RB,1 = 7837 × 109 Nmm; and 12 Nmm2 . RI,1 = 7587 × 10 The matrix F1 =

430.7 × 10−12 N−1

−444.8 × 10−15 N−1 mm−1

−444.8 × 10−15 N−1 mm−1

591.3 × 10−18 N−1 mm−2

.

Strain at reference axis and curvature: εr,1 = −405.1 × 10−6 and κ1 = −0.148 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε1(top) = −427.4 × 10−6 and ε1(btm) = −598.5 × 10−6 . Concrete stresses: σc(1),1(top) = −4.49 MPa and σc(1),0(btm) = −6.33 MPa. Reinforcement stresses: σs(2),1 = −87.3 MPa and σs(3),1 = −117.9 MPa. Stresses in tendons: σp(1),1 = 1231 MPa and σp(2),1 = 1231 MPa. The concrete stress resultants at τ1 = 40 days are: −1679 × 103 N . rc(1),1 = −1327 × 106 Nmm

Step 2: Short-term analysis at age τ = 40 days This step is identical to the previous one with the exception that the applied external load has increased due to the pour of the concrete deck. Strain at reference axis and curvature: εr,2 = −680.9 × 10−6 and κ2 = 0.217 × 10−6 mm−1 . Strains in the top and bottom ﬁbres of the I-section: ε2(top) = −648.2 × 10−6 and ε2(btm) = −397.7 × 10−6 . Concrete stresses: σc(1),2(top) = −11.56 MPa and σc(1),2(btm) = 0.09 MPa. Reinforcement stresses: σs(2),2 = −127.0 MPa and σs(3),2 = −82.1 MPa. Stresses in tendons: σp(1),2 = 1231 MPa and σp(2),2 = 1231 MPa. The concrete stress resultants at τ = 40 days after the wet concrete is poured are: −1708 × 103 N . rc(1),2 = −779.8 × 106 Nmm

Step 3: Grouting of tendons and commencement of composite action at age τ1 = 40 days During this step, the cross-sectional properties change due to the grouting of the tendons and due to the deck beginning to act compositely with the I-section. This change in cross-section will be captured in f set,j to ensure that the added components are unloaded at the time of setting. The cross-sectional properties of both I-section (element 1) and the concrete deck (element 2) are: Ac(1b) = 312.7 × 103 mm2 Bc(1b) = 234.2 × 106 mm3 Ic(1b) = 224.4 × 109 mm4

210 Uncracked sections Ac(2) = 357.3 × 103 mm2 Bc(2) = 26.79 × 106 mm3 Ic(2) = 2685 × 106 mm4 The cross-sectional rigidities are: RA,3 = 17,840 × 106 N RB,3 = 8852 × 109 Nmm; and RI,3 = 8179 × 1012 Nmm2 Matrix F3 is now: F3 =

121.1 × 10−12 N−1

−131.0 × 10−15 N−1 mm−1

−131.0 × 10−15 N−1

264.1 × 10−18 N−1 mm−1

The time-dependent effects of creep and shrinkage of the concrete and the relaxation response, that is, f cr,3 , f sh,3 and f p.rel,3 , are identical to those of the previous two steps as they all correspond to age 40 days. The vectors deﬁning the unloaded condition for the grout, prestressing and concrete deck at the time of setting are determined below. For prestressing cables and grout: Agrout = Aduct(1) + Aduct(2) − Apre(1) − Apre(2) = 2827 + 2827 − 800 − 800 = 4054 mm2 Bgrout = Bduct(1) + Bduct(2) − Bpre(1) − Bpre(2) = (2827 − 800) × 1030 + (2827 − 800) × 1160 = 4439.1 × 103 mm3 Igrout = Iduct(1) + Iduct(2) − Ipre(1) − Ipre(2) = (2827 − 800) × 10302 + (2827 − 800) × 11602 = 4877.9 × 106 mm4

Agrout Ec(1),3 εr,2 + Bgrout Ec(1),3 κ2 fc(1).set,3 = Bgrout Ec(1),3 εr,2 + Igrout Ec(1),3 κ2 ⎤ ⎡ 4054 × 32,000 × −680.9 × 10−6 + 4439.1 × 103 ⎥ ⎢ ⎥ ⎢ ×32,000 × 0.217 × 10−6 ⎥ ⎢ =⎢ ⎥ ⎣4439.1 × 103 × 32,000 × −680.9 × 10−6 + 4877.9 × 106 ⎦ ×32,000 × 0.217 × 10−6 −57.4 × 103 N = −62.7 × 106 Nmm

Uncracked sections 211

Ap(1) Ep(1) εr,2 + Bp(1) Ep(1) κ2 Bp(1) Ep(1) εr,2 + Ip(1) Ep(1) κ2 ⎤ ⎡ 800 × 200 × 103 × −680.9 × 10−6 + 800 × 1030 ⎥ ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎢ ⎥ =⎢ ⎥ 3 −6 2 + 800 × 1030 × −680.9 × 10 800 × 1030 × 200 × 10 ⎣ ⎦ ×200 × 103 × 0.217 × 10−6 −73.0 × 103 N = −75.2 × 106 Nmm Ap(2) Ep(2) εr,2 + Bp(2) Ep(2) κ2 fp(2).set,3 = Bp(2) Ep(2) εr,2 + Ip(2) Ep(2) κ2 ⎡ ⎤ 800 × 200 × 103 × −680.9 × 10−6 + 800 × 1160 ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎥ ⎥ =⎢ ⎢ ⎥ ⎣800 × 1160 × 200 × 103 × −680.9 × 10−6 + 800 × 11602 ⎦ ×200 × 103 × 0.217 × 10−6 −68.5 × 103 N = −79.5 × 106 Nmm

fp(1).set,3 =

For the concrete deck: Ac(2) Ec(2),3 εr,2 + Bc(2) Ec(2),3 κ2 fc(2),set,3 = Bc(2) Ec(2),3 εr,2 + Ic(2) Ec(2),3 κ2 ⎡ ⎤ 357,300 × 18,000 × −680.9 × 10−6 + 26.79 × 106 ⎢ ⎥ ⎢ ×18,000 × 0.217 × 10−6 ⎥ ⎢ ⎥ =⎢ ⎥ 6 −6 6 + 2685 × 10 ⎦ ⎣26.79 × 10 × 18,000 × −680.9 × 10 ×18,000 × 0.217 × 10−6 −4274 × 103 N = −317.9 × 106 Nmm As(1) Es(1) εr,2 + Bs(1) Es(1) κ2 fs(1).set,3 = Bs(1) Es(1) εr,2 + Is(1) Es(1) κ2 ⎤ ⎡ 2700 × 200 × 103 × −680.9 × 10−6 + 202.5 × 103 ⎥ ⎢ ⎥ ⎢ ×200 × 103 × 0.217 × 10−6 ⎢ ⎥ =⎢ ⎥ 3 3 −6 6 + 15.19 × 10 × 200 × 10 × −680.9 × 10 202.5 × 10 ⎣ ⎦ ×200 × 103 × 0.217 × 10−6 −358.8 × 103 N = −26.9 × 106 Nmm

212 Uncracked sections Combining the above contributions related to concrete setting: fset,3 = fc(1).set,3 + fp(1).set,3 + fp(2).set,3 + fc(2).set,3 + fs(1).set,3 −4832 × 103 N = −562.2 × 106 Nmm The strain distribution at time τ3 can then be determined as: ε3 = F3 re,3 − fcr,3 + fsh,3 − fp,init + fp.rel,3 + fset,3 0 121.1 × 10−12 −131.0 × 10−15 = × 1170 × 106 −131.0 × 10−15 264.1 × 10−18 2427 × 103 −987.7 × 103 2000 × 103 30 × 103 − + − + 1961 × 106 −735.3 × 106 2190 × 106 32.85 × 106 −4832 × 103 −680.9 × 10−6 + = −562.2 × 106 0.217 × 10−6 mm−1 As expected there is no change in deformation between steps 3 and 4 as the new cross-sectional components are kept unloaded. The strain diagram for the precast I-section at step 3 is identical to the one already calculated for step 2: ε3(top) = ε2(top) = −648.2 × 10−6 ε3(btm) = ε2(btm) = −397.7 × 10−6 Stresses at step 3 are also identical to those obtained at Step 2 as shown below: For the precast I-section: " # 1 yc(1),(top) ε3 − εsh(1),3 + Fe(1),3,0 σc(1),0(top) σc(1),3(top) = Ec(1),3 ! −680.9 × 10−6 = 32,000 1 150 − −100 × 10−6 0.217 × 10−6 − 1.304 × (−4.60) = −11.56 MPa " # 1 yc(1),(btm) ε3 − εsh(1),3 + Fe(1),3,0 σc(1),0(btm) σc(1),3(btm) = Ec(1),3 = 0.09 MPa For the concrete deck:

" # 1 yc(2),(top) ε3 − εsh(2),3 − Ec(2),3 1 yc(2),(top) ε2 ! −680.9 × 10−6 = 18,000 1 0 −0 0.217 × 10−6 ! −680.9 × 10−6 − 18,000 1 0 = 0.0 MPa 0.217 × 10−6

σc(2),3(top) = Ec(2),3

Uncracked sections 213 " # σc(2),3(btm) = Ec(2),3 1 yc(2),(btm) ε3 − εsh(2),3 − Ec(2),3 1 yc(2),(btm) ε2 = 0.0 MPa For the non-prestressed reinforcement:

3

σs(1),3 = 200 × 10 × 1 75

−680.9 × 10−6

−

0.217 × 10−6

−680.9 × 10−6

0.217 × 10−6

= 0.0 MPa

−680.9 × 10−6 σs(2),3 = 200 × 10 × 1 210 0.217 × 10−6

3

= −127.0 MPa

−680.9 × 10−6 σs(3),3 = 200 × 10 1 1240 0.217 × 10−6 3

= −82.1 MPa For the prestressing steel: σp(1),3 = Ep(1) 1 yp(1) (ε3 − ε2 ) + Ep(1) (εp(1),init − εp.rel(1),3 ) = 1231 MPa σp(2),3 = Ep(2) 1 yp(2) (ε3 − ε2 ) + Ep(2) (εp(2),init − εp.rel(2),3 ) = 1231 MPa The concrete stress resultants at step 3, τ = 40 days after the wet concrete has set, are: rc(1),3 = Dc(1),3 ε3 + fcr(1),3 − fsh(1),3 − fset(1),3 = rc(2),3 = Dc(2),3 ε3 + fcr(2),3 − fsh(2),3 − fset(2),3 =

−1708 × 103 N

−779.8 × 106 Nmm 0N 0 Nmm

Step 4: Time analysis SSM at age 60 days In step 4, the stresses and strains due to the previous loading history are evaluated at 60 days. The following cross-sectional properties are calculated for step 4: RA,4 = 20,960 × 106 N; RB,4 = 9508 × 109 Nmm; RI,4 = 8647 × 1012 Nmm2 .

214 Uncracked sections The matrix F4 is: F4 =

95.15 × 10−12 N−1

−104.6 × 10−15 N−1 mm−1

−104.6 × 10−15 N−1 mm−1

230.7 × 10−18 N−1 mm−2

The effects of creep and shrinkage in this time period are: fcr,4 = Fe(1),4,0 rc(1),0 + Fe(1),4,3 rc(1),3 −1862 × 103 −1708 × 103 = −0.807 × − 0.912 × −1504 × 106 −779.8 × 106 3061 × 103 N = 1925 × 106 Nmm

Ac(1) Ac(2) fsh,4 = Ec(1),4 εsh(1),4 + Ec(2),4 εsh(2),4 Bc(1) Bc(2)

357,300 312,700 −6 = × 34,000 × −150 × 10 + 234.2 × 106 26.79 × 106 × 25,000 × −200 × 10−6 −1786 × 103 −1595 × 103 −3381 × 103 N = + = −1328 × 106 Nmm −1195 × 106 −133.9 × 106 Note that the grout is assumed to be shrinking at the same rate as the concrete used for the precast I-section. The effects of relaxation of the steel tendon are calculated from Eq. 5.90f: fp.rel,4 =

Ap(1) Ep(1) εp(1),init ϕp (60, σp(1),init )

yp(1) Ap(1) Ep(1) εp(1),init ϕp (60, σp(1),init ) Ap(2) Ep(2) εp(2),init ϕp (60, σp(2),init ) 40 × 103 N + = yp(2) Ap(2) Ep(2) εp(2),init ϕp (60, σp(2),init ) 43.8 × 106 Nmm

The terms deﬁning f set,4 are calculated based on the corresponding values already obtained at time τ3 and adjusted for the change in elastic moduli that has taken place: −57.4×103 34,000 −61.0×103 N Ec(1),4 fc(1).set,4 = fc(1).set,3 = = Ec(1),3 −66.6×106 Nmm −62.7×106 32,000 −73.0×103 N fp(1).set,4 = fp(1).set,3 = −75.2×106 Nmm

fp(2).set,4 = fp(2).set,3 =

−68.5 × 103

−79.5 × 106

N

Uncracked sections 215

Nmm

−4274 × 103 Ec(2),4 = fc(2).set,4 = fc(2).set,3 Ec(2),3 −317.9 × 106 −5936 × 103 N = −441.5 × 106 Nmm −358.8 × 103 N fs(1).set,4 = fs(1).set,3 = −26.9 × 106 Nmm

25,000 18,000

fset,4 = fc(1).set,4 + fp(1).set,4 + fp(2).set,4 + fc(2).set,4 + fs(1).set,4 −6498 × 103 N = −689.8 × 106 Nmm The strain distribution at time τ4 becomes: ε4 = F4 re,4 − fcr,4 + fsh,4 − fp,init + fp.rel,4 + fset,4 0 95.15 × 10−12 −104.6 × 10−15 = × 1170 × 106 −104.6 × 10−15 230.7 × 10−18 3061 × 103 −3381 × 103 2000 × 103 40 × 103 − + − + 1925 × 106 −1328 × 106 2190 × 106 43.8 × 106 −6498 × 103 −903.0 × 10−6 + = −689.8 × 106 0.424 × 10−6 mm−1 At age 60 days, εr,4 = −903.0 × 10−6 and κ4 = 0.424 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to: ε4(top) = εr,4 + 150 × κ4 = −839.4 × 10−6 and ε4(btm) = εr,4 + 1300 × κ4 = −351.9 × 10−6 Stresses at the end of step 4 are calculated below: For the precast I-section: " # 1 yc(1),(top) ε4 − εsh(1),4 + Fe(1),4,0 σc(1),0(top) σc(1),4(top) = Ec(1),4 + Fe(1),4,3 σc(1),3(top) ! −903.0 × 10−6 −6 − −150 × 10 = 34,000 1 150 0.424 × 10−6 − 0.807 × (−4.60) − 0.912 × (−11.56) = −9.19 MPa

216 Uncracked sections and σc(1),4(btm) = Ec(1),4

" # 1 yc(1),(btm) ε4 − εsh(1),4 + Fe(1),4,0 σc(1),0(btm)

+ Fe(1),4,3 σc(1),3(btm) = −0.99 MPa For the concrete deck: " # 1 yc(2),(top) (ε4 − ε2 ) + Fe(2),4,3 σc(1),3(top) − εsh(2),4 −903.0 × 10−6 −680.9 × 10−6 = 25,000 1 0 − +0 0.424 × 10−6 0.217 × 10−6 ! − −200 × 10−6 = −0.55 MPa

σc(2),4(top) = Ec(2),4

" # 1 yc(2),(btm) (ε4 − ε2 ) + Fe(2),4,3 σc(1),3(btm) − εsh(2),4 −903.0 × 10−6 −680.9 × 10−6 = 25,000 1 150 − +0 0.424 × 10−6 0.217 × 10−6 ! −6 = 0.22 MPa − −200 × 10

σc(2),4(btm) = Ec(2),4

For the non-prestressed reinforcement: 3

σs(1),4 = 200 × 10 × 1 75

−903.0 × 10−6 0.424 × 10−6

−

−680.9 × 10−6 0.217 × 10−6

= −41.3 MPa

−903.0 × 10−6 σs(2),4 = 200 × 10 × 1 210 = −162.8 MPa 0.424 × 10−6 −6 −903.0 × 10 σs(3),4 = 200 × 103 1 1240 = −75.5 MPa 0.424 × 10−6 3

For the prestressing steel: σp(1),4 = Ep(1) 1 yp(1) (ε4 − ε2 ) + Ep(1) εp(1),init − εp.rel(1),4 −903.0 × 10−6 −680.9 × 10−6 3 = 200 × 10 × 1 1030 − 0.424 × 10−6 0.217 × 10−6 + 200,000 × 0.00625 × (1 − 0.02) = 1223 MPa

Uncracked sections 217 σp(2),4 = Ep(2) 1 yp(2) (ε4 − ε2 ) + Ep(2) εp(2),init − εp.rel(2),4 −6 −6 −680.9 × 10 −903.0 × 10 = 200 × 103 × 1 1160 − 0.424 × 10−6 0.217 × 10−6

+ 200,000 × 0.00625 × (1 − 0.02) = 1228 MPa The concrete stress resultants at step 4 at τ = 60 days are: rc(1),4 = Dc(1),4 ε4 + fcr(1),4 − fsh(1),4 − fc(1).set,4 312,700 234.2 × 106 −903.0 × 10−6 = 34,000 × 0.424 × 10−6 234.2 × 106 224.4 × 109 3061 × 103 −1595 × 103 −61.0 × 103 + − − 1925 × 106 −1195 × 106 −66.6 × 106 −1507 × 103 N = −769.1 × 106 Nmm rc(2),4 = Dc(2),3 ε4 + fcr(2),4 − fsh(2),4 − fc(2).set,4 −903.0 × 10−6 357,300 26.79 × 106 0 + = 25,000 × 6 −6 6 0 0.424 × 10 26.79 × 10 2685 × 10 −1786 × 103 −5936 × 103 −59.7 × 103 N − − = −0.999 × 106 Nmm −133.9 × 106 −441.5 × 106

Step 5: Time analysis SSM at age 60 days The cross-sectional properties, the creep and shrinkage of the concrete and relaxation of the prestressing tendons are identical to the previous step. The only change for step 5 is an additional external moment applied to the composite section. Based on the results calculated for step 4, the strain variables can be calculated by modifying vector re,5 to account for the change in external moment as: ε5 = F5 re,5 − fcr,5 + fsh,5 − fp,init + fp.rel,5 + fset,5 0 95.15 × 10−12 −104.6 × 10−15 = × 1570 × 106 −104.6 × 10−15 230.7 × 10−18 3061 × 103 −3381 × 103 2000 × 103 40 × 103 − + − + 1925 × 106 −1328 × 106 2190 × 106 43.8 × 106 −6498 × 103 −944.9 × 10−6 + = −689.8 × 106 0.516 × 10−6 mm−1

218 Uncracked sections At age 60 days, after the application of the road deck and other imposed dead loads, εr,5 = −944.9 × 10−6 and κ5 = 0.516 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to: ε5(top) = εr,5 + 150 × κ5 = −867.4 × 10−6 and ε5(btm) = εr,5 + 1300 × κ5 = −273.8 × 10−6 Stresses at the end of step 5 are calculated below: For the precast I-section: " # 1 yc(1),(top) ε5 − εsh(1),5 + Fe(1),5,0 σc(1),0(top) σc(1),5(top) = Ec(1),5 + Fe(1),5,3 σc(1),3(top) ! −944.9 × 10−6 = 34,000 1 150 − −150 × 10−6 0.516 × 10−6 − 0.807 × (−4.60) − 0.912 × (−11.56) = −10.14 MPa and σc(1),5(btm) = Ec(1),5

" # 1 yc(1),(btm) ε5 − εsh(1),5 + Fe(1),5,0 σc(1),0(btm)

+ Fe(1),5,3 σc(1),3(btm) = 1.66 MPa For the concrete deck:

" # 1 yc(2),(top) (ε5 − ε2 ) + Fe(2),5,3 σc(1),3(top) − εsh(2),5 −944.9 × 10−6 −680.9 × 10−6 = 25,000 1 0 − +0 0.516 × 10−6 0.217 × 10−6 ! −6 − −200 × 10 = −1.60 MPa

σc(2),5(top) = Ec(2),5

and σc(2),5(btm) = Ec(2),5

" # 1 yc(2),(btm) (ε5 − ε2 ) + Fe(2),5,3 σc(1),3(btm) − εsh(2),5

= −0.48 MPa For the non-prestressed reinforcement: −944.9 × 10−6 −680.9 × 10−6 3 σs(1),5 = 200 × 10 × 1 75 − 0.516 × 10−6 0.217 × 10−6 = −48.3 MPa

Uncracked sections 219

−944.9 × 10−6 σs(2),5 = 200 × 103 × 1 210 = −167.3 MPa 0.516 × 10−6 −944.9 × 10−6 3 σs(3),5 = 200 × 10 1 1240 = −60.9 MPa 0.516 × 10−6 For the prestressing steel: σp(1),5 = Ep(1) 1 yp(1) (ε5 − ε2 ) + Ep(1) εp(1),init − εp.rel(1),5 −944.9 × 10−6 −680.9 × 10−6 3 = 200 × 10 × 1 1030 − 0.516 × 10−6 0.217 × 10−6 + 200,000 × 0.00625 × (1 − 0.02) = 1234 MPa σp(2),5 = Ep(2) 1 yp(2) (ε5 − ε2 ) + Ep(2) εp(2),init − εp.rel(2),5 = 1241 MPa The concrete stress resultants at step 5 at τ = 60 days are: rc(1),5 = Dc(1),5 ε5 + fcr(1),5 − fsh(1),5 − fc(1).set,5 312,700 234.2 × 106 −944.9 × 10−6 = 34,000 × 0.516 × 10−6 234.2 × 106 224.4 × 109 3061 × 103 −1595 × 103 −61.0 × 103 + − − 1925 × 106 −1195 × 106 −66.6 × 106 −1217 × 103 N = −398.3 × 106 Nmm rc(2),5 = Dc(2),5 ε5 + fcr(2),5 − fsh(2),5 − fc(2).set,5 357,300 26.79 × 106 −944.9 × 10−6 0 = 25,000 × + 6 6 −6 0 0.516 × 10 26.79 × 10 2685 × 10 −1786 × 103 −5936 × 103 −371.7 × 103 N − − = −22.8 × 106 Nmm −133.9 × 106 −441.5 × 106

Step 6: Time analysis – SSM at age 30,000 days The cross-sectional rigidities for step 6 are: RA,6 = 24,000 × 106 N; RB,6 = 10,580 × 109 Nmm; RI,6 = 9558 × 1012 Nmm2 .

220 Uncracked sections The matrix F6 is: F6 =

81.35 × 10−12 N−1

−90.03 × 10−15 N−1 mm−1

−90.03 × 10−15 N−1 mm−1

204.2 × 10−18 N−1 mm−2

The effects of creep and shrinkage in this time period are: fcr,6 = Fe(1),6,0 rc(1),0 + Fe(1),6,3 rc(1),3 + Fe(1),6,5 rc(1),5 + Fe(2),6,5 rc(2),5 −1862 × 103 −1708 × 103 = −1.995 × − 0.419 × −1504 × 106 −779.8 × 106 −1217 × 103 −371.7 × 103 − 1.906 × − 3.56 × −398.3 × 106 −22.8 × 106 8074 × 103 N = 4167 × 106 Nmm

Ac(2) Ac(1) fsh,6 = Ec(1),6 εsh(1),6 + Ec(2),6 εsh(2),6 Bc(1) Bc(2) 357,300 312,700 −6 × 38,000 × −400 × 10 + = 26.79 × 106 234.2 × 106 × 30,000 × −600 × 10−6 −11,180 × 103 N = −4042 × 106 Nmm Relaxation of the steel tendon is accounted for using: fp.rel,6 =

2

Ap(i) Ep(i) εp(i),init ϕp (30,000, σp(i),init )

yp(i) Ap(i) Ep(i) εp(i),init ϕp (30,000, σp(i),init ) 800 × 200,000 800 × 200,000 = + 1030 × 800 × 200,000 1160 × 800 × 200,000 60.0 × 103 N × 0.00625 × 0.030 = 65.7 × 106 Nmm i=1

The terms deﬁning f set,6 are calculated using the same procedure adopted at time τ4 : −57.4 × 103 38,000 −68.1 × 103 N Ec(1),6 = = fc(1).set,6 = fc(1).set,3 Ec(1),3 −74.5 × 106 Nmm −62.7 × 106 32,000

fp(1).set,6 = fp(1).set,3 =

N

Uncracked sections 221

−75.2 × 106

fp(2).set,6 = fp(2).set,3 =

−73.0 × 103

Nmm −68.5 × 103 N

−79.5 × 106 Nmm −4274 × 103 30,000 Ec(2),6 fc(2).set,6 = fc(2).set,3 = Ec(2),3 −317.9 × 106 18,000 −7123 × 103 N = −529.8 × 106 Nmm −358.8 × 103 N fs(1).set,6 = fs(1).set,3 = −26.9 × 106 Nmm fset,6 = fc(1).set,6 + fp(1).set,6 + fp(2).set,6 + fc(2).set,6 + fs(1).set,6 −7692 × 103 N = −785.9 × 106 Nmm

The strain distribution at time τ6 becomes: ε6 = F6 re,6 − fcr,6 + fsh,6 − fp,init + fp.rel,6 + fset,6 0 81.35 × 10−12 −90.03 × 10−15 = × 1570 × 106 −90.03 × 10−15 204.2 × 10−18 8074 × 103 −11,180 × 103 2000 × 103 60.0 × 103 − + − + 4167 × 106 −4042 × 106 2190 × 106 65.7 × 106 −7692 × 103 −1490 × 10−6 + = −785.9 × 106 0.650 × 10−6 mm−1 At age 30,000 days, εr,6 = −1490 × 10−6 and κ6 = 0.650 × 10−6 mm−1 with strains in the top and bottom of the I-section equal to ε6(top) = −1393 × 10−6 and ε6(btm) = −644.8 × 10−6 . The strains in the top and bottom of the concrete deck are calculated as follows (measured from the time of setting): ε6,(top) = 1 0 (ε6 − ε2 ) = −809.5 × 10−6 ε6,(btm) = 1 150 (ε6 − ε2 ) = −744.6 × 10−6 Final stresses at time 30,000 days are calculated below: For the precast I-section: σc(1),6(top) = −4.40 MPa; σc(1),6(btm) = 2.21 MPa For the concrete deck: σc(2),6(top) = −0.59 MPa; σc(2),6(btm) = −2.63 MPa

222 Uncracked sections For the non-prestressed reinforcement: σs(1),6 = −155.4 MPa; σs(2),6 = −270.8 MPa; σs(3),6 = −136.8 MPa For the prestressing steel: σp(1),6 = 1140 MPa; σp(2),6 = 1151 MPa. The strains and stresses at times τ0 and τ6 are plotted in Fig. 5.22. −183.6

−4.60 −37.9

1250 1250

−57.9 −295.2 −7.38 Strain × 10−6 Stress (MPa) (a) Cross-section −427.4

(b) Step 0: At 7 days −648.9

−4.49

−11.56

−87.3

−127.0 1231

1231 −82.1

−117.9

1231 −6.33 Stress (MPa)

−598.5 Strain × 10−6

(c) Step 1: Age 40 days before slab deck is cast −222.1 −839.4 −191.2 −9.19

−0.55 −41.3

−162.8

−397.7 Strain × 10−6

1231 0.09 Stress (MPa)

(d) Steps 2 and 3: Age 40 days after deck is cast and tendons are grouted −264.0 −1.60 −867.4 −219.2 −10.14 −48.3 −167.3

0.22

1234

1223 −60.9

−75.5 −351.9 Strain × 10−6

1228 −0.99 Stress (MPa)

−273.8 Strain × 10−6

−809.5 −744.6

1241 1.66 Stress (MPa)

(f) Step 5: Age 60 days after road surface applied

(e) Step 4: Age 60 days before road surface applied −1393

−0.48

−155.4 −4.40 −270.8

−0.59 −2.63

1140 −136.8

1151 −644.8 2.21 Stress (MPa) Strain × 10−6 (g) Step 6: Age 30,000 days

Figure 5.22 Strain and stress distributions for Example 5.10.

Uncracked sections 223

5.8 References 1. Gilbert, R.I. (1988). Time Effects in Concrete Structures. Elsevier Science Publishers, Amsterdam. 2. Ghali, A., Favre, R. and Eldbadry, M. (2002). Concrete Structures: Stresses and Deformations. Third edition, Spon Press, London. 3. Standards Australia (2004). Australian Standard for Bridge Design – Part 5: Concrete (AS5100.5–2004). Sydney, Australia. 4. Bazant, Z.P. and Wu, S.T. (1973). Dirichlet series creep function for aging concrete. Journal of the Engineering Mechanics Division, ASCE, 99(2), 367–387. 5. Bazant, Z.P. and Wu, S.T. (1974). Rate-type creep law of aging concrete based on Maxwell chain. Materials and Structures (RILEM), 7(37), 45–60. 6. Bradford, M.A. and Gilbert, R.I. (1992). Composite beams with partial interaction under sustained loads. Journal of Structural Engineering, ASCE, 118(7), 1871–1883. 7. Tarantino, A.M. and Dezi, L. (1992). Creep effects in composite beams with ﬂexible shear connectors. Journal of Structural Engineering, ASCE, 118(8), 2063–2081. 8. Dezi, L. and Tarantino, A.M. (1993). Creep in composite continuous beams-I: theoretical treatment. Journal of Structural Engineering, ASCE, 119(7), 2095–2111. 9. Gilbert, R.I. and Bradford, M.A. (1995). Time-dependent behaviour of continuous composite beams at service loads. Journal of Structural Engineering, ASCE, 121(2), 319–327. 10. Ranzi, G. and Bradford, M.A. (2006). Analytical solutions for the time-dependent behaviour of composite beams with partial interaction. International Journal of Solids and Structures, 43, 3770–3793. 11. Ranzi, G. and Bradford, M.A. (2009). Analysis of composite beams with partial interaction using the direct stiffness approach for time effects. International Journal for Numerical Methods in Engineering, 78, 564–586.

6

Uncracked sections Axial force and biaxial bending

6.1 Introduction Methods of analysis to evaluate the short- and long-term response of concrete crosssections subjected to axial force and biaxial bending are presented in this chapter. These methods are particularly useful for the analysis of reinforced, prestressed or composite steel-concrete columns in building structures. The concrete is assumed to remain uncracked and be able to carry any applied tension. The proposed formulation relies on the Euler–Bernoulli beam assumptions which require plane sections to remain plane and perpendicular to the member axis before and after deformation. As for the case of axial loading and uniaxial bending (Chapter 5), the governing system of equations describing the structural response is expressed as a function of the unknown variables required to deﬁne the strain diagram. For the case of biaxial bending, the strain diagram is deﬁned in terms of three variables, speciﬁcally the strain measured at the origin of the adopted orthogonal co-ordinate system εr and the curvatures calculated with respect to the two orthogonal x- and y-axes, κx and κy , respectively (as illustrated in Fig. 6.1). The external actions applied to the cross-section may include an axial force applied at the origin Ne and bending moments Mxe and Mye applied with respect to the x- and y-axes, respectively. As shown in Fig. 6.1b, the ﬂexural action is equivalent to an external moment Me applied at an angle θM . The strain at an arbitrary point on the cross-section can be calculated from: ε = εr + yκx − xκy

(6.1)

The negative sign placed before the third term in Eq. 6.1 is a consequence of the sign convention adopted for the applied moments (as illustrated in Fig. 6.1b). The three variables deﬁning the strain diagrams, i.e. εr , κx and κy , are determined by enforcing horizontal and rotational equilibrium on the cross-section: Ne = Ni

(6.2a)

Mxe = Mxi

(6.2b)

Mye = Myi

(6.2c)

Uncracked sections 225 er x

e kx

y

qM

x Mxe

y x

er

y

ky e (a) Generic cross-section and strain diagram

Me

Mye

(b) Applied moments

Figure 6.1 Typical section, strain distribution and sign convention for applied moments.

where Ni , Mxi and Myi are the internal actions resisted by the cross-section, i.e. axial force and moments with respect to the x- and y-axes, respectively, and are deﬁned as: (6.3a) Ni = σ dA A

Mxi =

yσ dA A

(6.3b)

Myi = −

xσ dA

(6.3c)

A

The negative sign included in the expression for Myi has been introduced to match the sign convention adopted for the external moment Mye (see Fig. 6.1b). It is useful to evaluate the angle of inclination θM of the applied moment Me measured from the x-axis (adopting clockwise rotations to be positive) using: tan θM =

Mye Mxe

(6.4)

The values of the three unknowns (εr , κx and κy ) are obtained by enforcing equilibrium (Eq. 6.2), with the strain over the section expressed by Eq. 6.1 (i.e. strain compatibility) and using the appropriate constitutive relationships in the calculation of the internal stresses and actions. For ease of notation, the derivations presented in the following are applicable to generic reinforced and prestressed concrete cross-sections, while other types of crosssections could be easily considered, for example, the composite sections considered in Chapter 5. The reinforced or prestressed concrete cross-section is assumed to contain ms reinforcing bars and mp prestressing tendons. Each steel reinforcing bar is identiﬁed by its area, elastic modulus and location with respect to both x- and y-axes, As(i) , Es(i) , xs(i) and ys(i) , respectively. The corresponding properties for the prestressing tendons are Ap(i) , Ep(i) , xp(i) and yp(i) , respectively.

226 Uncracked sections The required geometric properties of the concrete part of the cross-section are its area Ac , its ﬁrst moments of area with respect to both x- and y-axes Bxc and Byc , respectively, the corresponding second moments of area Ixc and Iyc , and the product moment of area Ixyc . Due to the similarities between the derivations proposed in this chapter and those already described in Chapter 5, reference to the latter chapter will be carried out extensively in the following to avoid unnecessary repetition. As in Chapter 5, the proposed procedure is quite general and can be applied with both linear and nonlinear material models, even though in the latter case the integrals of Eq. 6.3 might need to be evaluated numerically.

6.2 Short-term analysis The short-term analysis of a reinforced or prestressed concrete cross-section subjected to axial force and biaxial bending is similar to that already described for uniaxial bending in Chapter 5, with the only addition being that moment equilibrium is enforced with respect to both the x- and y-axes. Based on linear-elastic material properties (Eq. 5.4), the axial equilibrium equation (Eq. 6.2a) can be expressed similarly to Eq. 5.6: Ne,0 = Ni,0 = Nc,0 + Ns,0 + Np,0

(6.5)

As in Chapter 5, the subscript ‘0’ indicates that all variables are calculated at time τ0 before any creep and shrinkage has taken place. In the case of axial force and biaxial bending, Nc,0 , Ns,0 and Np,0 may be expressed in terms of the strain distribution of Eq. 6.1 as: Nc,0 =

σc,0 dA =

Ac

Ec,0 εr,0 + yκx,0 − xκy,0 dA

Ac

= Ac Ec,0 εr,0 + Bxc Ec,0 κx,0 − Byc Ec,0 κy,0 Ns,0 =

ms

(6.6a)

As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0

i=1

= RA,s εr,0 + RBx,s κx,0 − RBy,s κy,0 Np,0 =

(6.6b)

mp Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

mp = RA,p εr,0 + RBx,p κx,0 − RBy,p κy,0 + Ap(i) Ep(i) εp(i),init

(6.6c)

i=1

where RA,s and RA,p represent the axial rigidity of the non-prestressed steel and prestressing tendons, respectively, and RBx,s and RBy,s (RBx,p and RBy,p ) are the ﬁrst moments of the rigidity of the steel reinforcement (prestressing tendons) with respect

Uncracked sections 227 to the x- and y-axes, respectively, and are given by: RA,s =

ms As(i) Es(i)

(6.7a)

i=1 ms RBx,s = ys(i) As(i) Es(i)

(6.7b)

i=1

RBy,s =

ms xs(i) As(i) Es(i)

(6.7c)

i=1 mp RA,p = Ap(i) Ep(i)

(6.7d)

i=1 mp RBx,p = yp(i) Ap(i) Ep(i)

(6.7e)

i=1 mp RBy,p = xp(i) Ap(i) Ep(i)

(6.7f)

i=1

In a similar way, moment equilibrium with respect to the x-axis is enforced using Eq. 6.2b as: Mxe,0 = Mxi,0 = Mxc,0 + Mxs,0 + Mxp,0

(6.8)

in which the internal actions are calculated using: Mxc,0 =

yσc,0 dA =Bxc Ec,0 εr,0 + Ixc Ec,0 κx,0 − Ixyc Ec,0 κy,0

(6.9a)

Ac ms Mxs,0 = ys(i) As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0 i=1

= RBx,s εr,0 + RIx,s κx,0 − RIxy,s κy,0 Mxp,0 =

(6.9b)

mp yp(i) Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

= RBx,p εr,0 + RIx,p κx,0 − RIxy,p κy,0 +

mp yp(i) Ap(i) Ep(i) εp(i),init

(6.9c)

i=1

and RIx,s and RIy,s (RIx,p and RIy,p ) are the rigidities associated with the second moments of area of the steel reinforcement (prestressing tendons) with respect to the

228 Uncracked sections x- and y-axes, respectively, and are given by: ms 2 ys(i) As(i) Es(i) RIx,s =

(6.10a)

i=1

RIxy,s =

ms xs(i) ys(i) As(i) Es(i)

(6.10b)

i=1 mp 2 RIx,p = yp(i) Ap(i) Ep(i)

(6.10c)

i=1 mp RIxy,p = xp(i) yp(i) Ap(i) Ep(i)

(6.10d)

i=1

Finally, considering ﬂexural equilibrium with respect to the y-axis (Eq. 6.2c) gives: Mye,0 = Myi,0 = Myc,0 + Mys,0 + Myp,0 where:

(6.11)

Myc,0 = −

xσc,0 dA = − Byc Ec,0 εr,0 − Ixyc Ec,0 κx,0 + Iyc Ec,0 κy,0

(6.12a)

Ac

Mys,0 = −

ms xs(i) As(i) Es(i) εr,0 + ys(i) κx,0 − xs(i) κy,0 i=1

= −RBy,s εr,0 − RIxy,s κx,0 + RIy,s κy,0

(6.12b)

mp

Myp,0 = −

xp(i) Ap(i) Ep(i) εr,0 + yp(i) κx,0 − xp(i) κy,0 + εp(i),init i=1

mp = −RBy,p εr,0 − RIxy,p κx,0 + RIy,p κy,0 − xp(i) Ap(i) Ep(i) εp(i),init

(6.12c)

i=1

and RIy,s =

ms x2s(i) As(i) Es(i)

(6.13a)

i=1 mp RIy,p = x2p(i) Ap(i) Ep(i)

(6.13b)

i=1

Eqs 6.5, 6.8 and 6.11 can be therefore re-written as: mp Ap(i) Ep(i) εp(i),init Ne,0 = RA,0 εr,0 + RBx,0 κx,0 − RBy,0 κy,0 + i=1

(6.14a)

Uncracked sections 229 mp

Mxe,0 = RBx,0 εr,0 + RIx,0 κx,0 − RIxy,0 κy,0 +

yp(i) Ap(i) Ep(i) εp(i),init

(6.14b)

i=1

Mye,0 = −RBy,0 εr,0 − RIxy,0 κx,0 + RIy,0 κy,0 −

mp xp(i) Ap(i) Ep(i) εp(i),init

(6.14c)

i=1

where the cross-sectional rigidities are given by: RA,0 = Ac Ec,0 + RA,s + RA,p

(6.15a)

RIxy,0 = Ixyc Ec,0 + RIxy,s + RIxy,p

(6.15b)

RBx,0 = Bxc Ec,0 + RBx,s + RBx,p

(6.15c)

RBy,0 = Byc Ec,0 + RBy,s + RBy,p

(6.15d)

RIx,0 = Ixc Ec,0 + RIx,s + RIx,p

(6.15e)

RIy,0 = Iyc Ec,0 + RIy,s + RIy,p

(6.15f)

This governing system of equations (Eqs 6.14) can be expressed in compact form as: re,0 = D0 ε0 + fp,init

(6.16)

and using notation similar to that adopted in Chapter 5: ⎡ ⎤ Ne,0 re,0 = ⎣ Mxe,0 ⎦ Mye,0 ⎡ ⎤ RA,0 RBx,0 −RBy,0 D0 = ⎣ RBx,0 RIx,0 −RIxy,0 ⎦ −RBy,0 −RIxy,0 RIy,0 ⎡ ⎤ εr,0 ε0 = ⎣ κx,0 ⎦ κy,0 ⎡ ⎤ mp Ap(i) Ep(i) ⎣ yp(i) Ap(i) Ep(i) ⎦ εp(i),init fp,init = i=1 −xp(i) Ap(i) Ep(i)

(6.17a)

(6.17b)

(6.17c)

(6.17d)

The unknown strain vector ε0 is obtained by solving Eq. 6.16 and is given by: re,0 − fp,init = F0 re,0 − fp,init (6.18) ε0 = D−1 0 in which ⎡ RIx,0 RIy,0 −R2Ixy,0 1 ⎢ F0 = ⎣RBy,0 RIxy,0 −RBx,0 RIy,0 R0 RBy,0 RIx,0 −RBx,0 RIxy,0

RBy,0 RIxy,0 −RBx,0 RIy,0 RA,0 RIy,0 −R2By,0 RA,0 RIxy,0 −RBx,0 RBy,0

⎤ RBy,0 RIx,0 −RBx,0 RIxy,0 ⎥ RA,0 RIxy,0 −RBx,0 RBy,0 ⎦ 2 RA,0 RIx,0 −RBx,0 (6.19a)

230 Uncracked sections and R0 = RA,0 RIx,0 RIy,0 − R2Ixy,0 − R2Bx,0 RIy,0 + 2RBx,0 RBy,0 RIxy,0 − R2By,0 RIx,0 (6.19b) The strain at any point (x, y) is obtained by substituting Eq. 6.18 into Eq. 6.1: ε0 = εr,0 + yκx,0 − xκy,0 = 1 y −x ε0

(6.20)

and the stress at any point can then be determined from the calculated strain (Eq. 6.20) using the appropriate constitutive relationship (Eqs 5.4). By setting Eq. 6.20 equal to zero, the equation of the line (in the x-y plane) deﬁning the neutral axis may be expressed as y=

κy,0 εr,0 x− κx,0 κx,0

(6.21)

Equation 6.21 is not deﬁned when κx,0 = 0, in which case the problem degenerates to one of axial force and uniaxial bending about the y-axis and can be solved using the methods of Chapter 5. The slope of the neutral axis at time τ0 may be obtained by differentiating Eq. 6.21 and (adopting clockwise rotations to be positive similarly to θM,0 ) is expressed as a function of the applied moments and ﬂexural rigidities: tan θNA,0 =

κy,0 κx,0

(6.22)

The neutral axis (Eq. 6.21) intersects the y-axis at: y(x = 0) = −

εr,0 κx,0

(6.23)

If the cross-section is doubly-symmetric (as is often the case in practice), the expression for F0 can be simpliﬁed by placing the origin of the coordinate system at the centroid of the cross-section and specifying the orthogonal axes to be parallel to the axes of symmetry (leading to RIxy,0 = RBx,0 = RBy,0 = 0). Therefore: ⎡

RIx,0 RIy,0 ⎣ 0 F0 = RA,0 RIx,0 RIy,0 0 1

0 RA,0 RIy,0 0

⎤ 0 ⎦ 0 RA,0 RIx,0

(6.24)

Without prestressing (usually the case for columns), using Eq. 6.24 in Eq. 6.18, the expression for the strain at a point ε0 simpliﬁes to: ε0 = εr,0 + yκx,0 − xκy,0 =

Mye,0 Ne,0 Mxe,0 +y −x RA,0 RIx,0 RIy,0

(6.25)

Uncracked sections 231 In this particular case (i.e. no prestressing), the equation of the line (in the x-y plane) deﬁning the neutral axis may be expressed in terms of external loads as: y=

RIx,0 Ne,0 RIx,0 Mye,0 x− RIy,0 Mxe,0 RA,0 Mxe,0

(6.26)

with corresponding slope and intersect with the y-axis calculated using: tan θNA,0 =

RIx,0 Mye,0 RIx,0 = tan θM,0 RIy,0 Mxe,0 RIy,0

(6.27a)

and y(x = 0) = −

RIx,0 Ne,0 RA,0 Mxe,0

(6.27b)

Evidently, the angle of the applied moment Me,0 (i.e. θM,0 ) and of the neutral axis (i.e. θNA,0 ) coincide only when the ﬂexural rigidities calculated with respect to both the x- and y-axes are identical, i.e. when RIx,0 = RIy,0 (Eq. 6.27a). In all other cases, these two angles differ from each other (Fig. 6.2). Moreover, the angle of the neutral axis θNA,0 may vary with time, as will be seen subsequently. The cross-sectional rigidities could have also been calculated from the transformed section, where the areas of the reinforcing bars and bonded prestressing tendons (As(i) and Ap(i) , respectively) are transformed into equivalent areas of concrete (ns(i),0 As(i) and np(i),0 Ap(i) , respectively), where ns(i),0 = Es(i) /Ec,0 is the modular ratio of the i-th steel bar and np(i),0 = Ep(i) /Ec,0 is the modular ratio of the i-th tendon. In this case, the cross-sectional rigidities are given by: RA,0 = A0 Ec,0

(6.28a)

RBx,0 = Bx,0 Ec,0

(6.28b)

RBy,0 = By,0 Ec,0

(6.28c)

RIx,0 = Ix,0 Ec,0

(6.28d)

RIy,0 = Iy,0 Ec,0

(6.28e)

RIxy,0 = Ixy,0 Ec,0

(6.28f)

x

Mxe,0

x

qM,0

qNA,0 er,0

y Mye,0 (a) Orientation of Me

Neutral axis

Me,0 y

(b) Orientation of the neutral axis

Figure 6.2 Orientations of applied moments and neutral axis.

k0

e

232 Uncracked sections where A0 is the area of the transformed concrete section; Bx,0 and Ix,0 are the transformed ﬁrst and second moments of area calculated with respect to the x-axis, respectively; By,0 and Iy,0 represent the corresponding moments of area with respect to the y-axis; and Ixy,0 is the product moment of area. Using Eqs 6.28, the matrix F0 , previously introduced in Eq. 6.19a, can be expressed as: ⎡

2 Ix,0 Iy,0 −Ixy,0 1 ⎢ F0 = ⎣ By,0 Ixy,0 −Bx,0 Iy,0 S0 Ec,0 By,0 Ix,0 −Bx,0 Ixy,0

By,0 Ixy,0 −Bx,0 Iy,0 A0 Iy,0 −B2y,0 A0 Ixy,0 −Bx,0 By,0

⎤ By,0 Ix,0 −Bx,0 Ixy,0 ⎥ A0 Ixy,0 −Bx,0 By,0 ⎦ A0 Ix,0 −B2x,0 (6.29a)

and 2 − B2x,0 Iy,0 + 2Bx,0 By,0 Ixy,0 − B2y,0 Ix,0 S0 = A0 Ix,0 Iy,0 − Ixy,0

(6.29b)

Considering the particular case of a doubly-symmetric section with the origin at the centroid of the section and orthogonal axes parallel to the axes of symmetry (for which RIxy,0 = RBx,0 = RBy,0 = 0), F0 simpliﬁes to: ⎡ Ix,0 Iy,0 1 ⎣ 0 F0 = A0 Ix,0 Iy,0 Ec,0 0

0 A0 Iy,0 0

⎤ 0 ⎦ 0 A0 Ix,0

(6.30)

Without prestressing effects, the strain at any point (x, y) can be calculated using: ε0 = εr,0 + yκx,0 − xκy,0 =

Mye,0 Ne,0 Mxe,0 +y −x A0 Ec,0 Ix,0 Ec,0 Iy,0 Ec,0

(6.31)

By setting ε0 = 0 in Eq. 6.31, the equation of the neutral axis, its slope and its intersection with the y-axis are obtained as functions of the transformed second moments of area and are given by: y= tan θNA,0 =

Ix,0 Ne,0 Ix,0 Mye,0 x− Iy,0 Mxe,0 A0 Mxe,0

(6.32a)

Ix,0 tan θM,0 Iy,0

(6.32b)

Ix,0 Ne,0 A0 Mxe,0

(6.32c)

y(x = 0) = −

As discussed in Chapter 5, the calculation of the cross-sectional rigidities based on the transformed section using Eqs 6.28 is equivalent to calculation using Eqs 6.15. Either approach can be used depending on the preference of the structural designer.

Uncracked sections 233

Example 6.1 The doubly-symmetric reinforced concrete cross-section shown in Fig. 6.3 is subjected to biaxial bending, with Mxe = 5 kNm and Mye = 10 kNm. In this example, the axial force is zero (i.e. Ne,0 = 0 kN). The stress and strain distributions are to be determined at time τ0 , assuming the origin of the coordinate system is located at the centroid of the cross-section and the x- and y-axes are parallel to the axes of symmetry (i.e. dx.ref = b/2 and dy.ref = D/2 measured from the left and top of the section, respectively, as shown in Fig. 6.3). Both concrete and reinforcement are assumed to be linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = ns(j),0 = Es /Ec,0 = 6.25 (with j = 1, . . ., 4). b = 300 dx.ref = 150 As(1) = 450 mm2

150

90

90 As(2) = 450 mm2

dy.ref = 150 90

x

D = 300

As(3) = 450 mm2

90 150

As(4) = 450 mm2

y

Figure 6.3 Reinforced concrete cross-section for Example 6.1 (dimensions in mm).

Based on the adopted reference system the coordinates of each of the four steel reinforcing bars are: xs(1) = −90 mm ys(1) = −90 mm xs(2) = 90 mm ys(2) = −90 mm xs(3) = 90 mm ys(3) = 90 mm xs(4) = −90 mm ys(4) = 90 mm For this reinforced concrete section, the vectors re,0 and f p,init are ⎤ ⎡ ⎡ ⎤ 0N 0N re,0 = ⎣ 5 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 10 × 106 Nmm

234 Uncracked sections Based on the transformed section, the relevant cross-sectional properties are calculated as: A0 = bD+(ns,0 −1)[As(1) +As(2) +As(3) +As(4) ] = 300×300+(6.25−1)×(4×450) = 99,450 mm2 ;

2 bD3 D 2 2 2 Ix,0 = +As(2) ys(2) +As(3) ys(3) +bD −dy.ref +(ns,0 −1) As(1) ys(1) 12 2 300×3003 2 +As(4) ys(4) = +3002 (150−150)2 12 +5.25×[2×450×(−90)2 +2×450×902 ] = 751.5×106 mm4 . From the double symmetry and the adopted coordinate system: Iy,0 = Ix,0 = 751.5 × 106 mm4 and Bx,0 = By,0 = Ixy,0 = 0. From Eq. 6.30: ⎡ ⎤ Ix,0 Iy,0 0 0 1 ⎢ ⎥ F0 = 0 A0 Iy,0 0 ⎣ ⎦ A0 Ix,0 Iy,0 Ec,0 0 0 A0 Ix,0 1 99,450×(751.5×106 ) 2 × 32,000 ⎤ ⎡ 2 6 751.5×10 0 0 ⎥ ⎢ ⎥ ×⎢ 0 99,450×751.5×106 0 ⎦ ⎣ 0 0 99,450×751.5×106 ⎤ ⎡ 3.142×10−10 N−1 0 0 ⎥ ⎢ =⎣ 0 4.158×10−14 N−1 mm−2 0 ⎦ 0 0 4.158×10−14 N−1 mm−2 =

The strain ε0 is then determined based on Eq. 6.18: ⎤ ⎡ 3.142 × 10−10 0 0 ⎦ ε0 = F0 re,0 − fp,init = ⎣ 0 4.158 × 10−14 0 0 0 4.158 × 10−14 ⎧⎡ ⎤ ⎡ ⎤⎫ 0 0 ⎬ ⎨ × ⎣ 5 × 106 ⎦ − ⎣ 0 ⎦ ⎭ ⎩ 0 10 × 106 ⎤ ⎡ 0 = ⎣ 0.208 × 10−6 mm−1 ⎦ 0.416 × 10−6 mm−1

Uncracked sections 235 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = 0 κx,0 = 0.208 × 10−6 mm−1 κy,0 = 0.416 × 10−6 mm−1 and, from Eq. 6.1, the strains at the corners of the cross-section become: ε0 (x = −b/2, y = −D/2) = (0 − 150 × 0.208 − (−150) × 0.416) × 10−6 = 31.2 × 10−6 ε0 (x = b/2, y = −D/2) = (0 − 150 × 0.208 − 150 × 0.416) × 10−6 = −93.6 × 10−6 ε0 (x = b/2, y = D/2) = (0 + 150 × 0.208 − 150 × 0.416) × 10−6 = −31.2 × 10−6 ε0 (x = −b/2, y = D/2) = (0 + 150 × 0.208 − (−150) × 0.416) × 10−6 = 93.6 × 10−6 The stresses in the concrete at the four corners of the cross-section are obtained from Eq. 5.16a: σc,0(top-left) = Ec,0 ε0(top-left) = 32 × 103 × 31.2 × 10−6 = 1.00 MPa σc,0(top-right) = −2.99 MPa σc,0(btm-right) = −1.00 MPa σc,0(btm-left) = 2.99 MPa Similarly, the stress in each reinforcement bar is calculated using Eq. 5.16b: σs(1),0 = Es 1 ys(1) −xs(1) ε0 ⎡ ⎤ 0 = 200 × 103 × [1 − 90 − (−90)] × ⎣ 0.208 × 10−6 ⎦ 0.416 × 10−6 = 3.7 MPa; σs(2),0 = −11.2 MPa σs(3),0 = −3.7 MPa σs(4),0 = 11.2 MPa The slopes of both applied moment Me and of the neutral axis are calculated as (Eqs 6.4 and 6.32b): tan θM,0 = tan θNA,0 =

Mye,0 10 × 106 = = 2.0 from which θM,0 = 63.43◦ and Mxe,0 5 × 106 Ix,0 751.5 × 106 tan θM,0 = × 2.0 = 2.0 Iy,0 751.5 × 106 and therefore θNA,0 = 63.43◦ .

As expected, θM,0 = θNA,0 because Ix,0 = Iy,0 .

236 Uncracked sections The strain and stress distributions are plotted in Fig. 6.4. The cross-sectional rigidities could have also been calculated based on Eqs 6.15: RA,0 = 3182 × 106 N RIx,0 = RIy,0 = 24.05 × 1012 Nmm2 RBx,0 = RBy,0 = RIxy,0 = 0 In this case, F0 is obtained from Eq. 6.24 and is identical to that calculated above.

x 63.43°

Neutral axis

−93.6 × 10−6

y

−2.99

e −11.2

93.6 × 10−6 −3.7 3.7 2.99

s

11.2

Figure 6.4 Initial strain and stress diagrams at time τ0 for Example 6.1 (all units in mm, MPa).

Example 6.2 The strain and stress distributions on the reinforced concrete cross-section shown in Fig. 6.5 are to be determined at time τ0 when the applied actions, Ne = −500 kN (compression), Mxe = 25 kNm and Mye = 25 kNm, are ﬁrst applied. The origin of the coordinate system is taken at the centroid of the section and the x- and y-axes are assumed to be parallel to the axes of symmetry (i.e. dx.ref = b/2 and dy.ref = D/2 measured from the left and top of the section, respectively).

Uncracked sections 237 The material behaviour is linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for all reinforcement is therefore ns,0 = Es /Ec,0 = 6.25. b = 300 dx.ref = 150

As(j) = 450 mm2

150

90

for j = 1,…,6

90

As(2)

As(1)

dy.ref = 200 150 x D = 400

As(4)

As(3)

150 200 As(5)

As(6) y

Figure 6.5 Reinforced concrete cross-section for Example 6.2 (dimensions in mm).

Based on the adopted reference system, the coordinates of the steel reinforcement are: xs(1) = −90 mm ys(1) = −150 mm xs(2) = 90 mm ys(2) = −150 mm xs(3) = −90 mm ys(3) = 0 mm xs(4) = 90 mm ys(4) = 0 mm xs(5) = −90 mm ys(5) = 150 mm xs(6) = 90 mm ys(6) = 150 mm The vectors of external loads and prestressing are: ⎡ ⎡ ⎤ ⎤ −500 × 103 N 0N re,0 = ⎣ 25 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 25 × 106 Nmm The properties of the transformed cross-section are: A0 = bD + (ns,0 − 1)

6 0 i=1

As(i) = 134.1 × 103 mm2

238 Uncracked sections

2 6 0 bD3 D 2 = 1812 × 106 mm4 Ix,0 = + bD − dy.ref + (ns,0 − 1) As(i) ys(i) 12 2 i=1

2 6 0 Db3 b Iy,0 = + bD − dx.ref + (ns,0 − 1) As(i) x2s(i) = 1014 × 106 mm4 12 2 i=1 For this cross-section and for these coordinate axes: Bx,0 = By,0 = Ixy,0 = 0. From Eq. 6.30: ⎡

⎤ 2.329×10−10 N−1 0 0 ⎢ ⎥ F0 = ⎣ 0 1.724×10−14 N−1 mm−2 0 ⎦ 0 0 3.080×10−14 N−1 mm−2

and ε0 is calculated using Eq. 6.18: ⎡ ⎤ −116.4 × 10−6 ε0 = F0 re,0 − fp,init = ⎣ 0.431 × 10−6 mm−1 ⎦ 0.770 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = −116.4 × 10−6 κx,0 = 0.431 × 10−6 mm−1 κy,0 = 0.770 × 10−6 mm−1 . The strains at the four corners of the cross-section are (Eq. 6.1): ε0(top-left) (x = −b/2, y = −D/2) = −87.2 × 10−6 ε0(top-right) (x = b/2, y = −D/2) = −318.1 × 10−6 ε0(btm-right) (x = b/2, y = D/2) = −145.7 × 10−6 ε0(btm-left) (x = −b/2, y = D/2) = 85.2 × 10−6 and the concrete and steel stress distributions are calculated using Eq. 5.16: σc,0(top-left) = Ec,0 ε0(top-left) = −2.79 MPa σc,0(top-right) = −10.18 MPa σc,0(btm-right) = −4.66 MPa σc,0(btm-left) = 2.73 MPa σs(1),0 = Es 1 ys(1) −xs(1) ε0 ⎡ ⎤ −116.4 × 10−6 = 200 × 103 × [1 − 150 − (−90)] × ⎣ 0.431 × 10−6 ⎦ 0.770 × 10−6 = −22.4 MPa; σs(2),0 = −50.1 MPa

Uncracked sections 239 σs(3),0 = −9.4 MPa σs(4),0 = −37.1 MPa σs(5),0 = 3.50 MPa σs(6),0 = −24.2 MPa The slopes of both applied moment Me,0 and of the neutral axis are (Eqs 6.4 and 6.32b): tan θM,0 =

tan θNA,0 =

Mye,0 25 × 106 = = 1.0 and therefore θM,0 = 45◦ and Mxe,0 25 × 106 Ix,0 1812 × 106 tan θM = × 1 = 1.79 Iy,0 1014 × 106 and therefore θNA,0 = 60.76◦ .

The calculated stresses and strains are shown in Fig. 6.6.

60.76°

x

Neutral axis

45° Me,0

−318.1 × 10−6

y

−10.18 e

85.2 × 10−6

−9.4

−37.1 −24.2 −22.4

−50.1

3.5 2.73

s

Figure 6.6 Initial strain and stress diagrams at time τ0 for Example 6.2 (all units in mm, MPa).

240 Uncracked sections In this case θM,0 = θNA,0 (since Ix,0 = Iy,0 ), and the neutral axis passes through the y-axis at (Eq. 6.32c): y=−

1812 × 106 −500 × 103 Ix,0 Ne,0 =− = 270.2 mm A0 Mxe,0 134.1 × 103 25 × 106

The cross-sectional rigidities could have also been calculated based on Eqs 6.15: RA,0 = 4293 × 106 N RIx,0 = 58 × 1012 Nmm2 RIy,0 = 32.47 × 1012 Nmm2 RBx,0 = RBy,0 = RIxy,0 = 0 In this case, F0 is obtained from Eq. 6.24 and is identical to that calculated above.

Example 6.3 For the reinforced concrete cross-section shown in Fig. 6.7, the strain and stress distributions are to be calculated at time τ0 . The section is subjected to: Ne = −800 kN (compression), Mxe = 50 kNm and Mye = 25 kNm. The origin b = 480

As(j) = 450 mm2 for j = 1, .. ,8

dx.ref = 215.6

1

60

180

180

60

2 60

As(2)

As(1)

As(3) D1 = 300

dy.ref = 215.6

180 x D = 480 As(4)

As(5)

As(6)

4

b2 = 180

3

60

120 D2 = 180

As(7)

As(8)

6

60

5 b1 = 300 y

Figure 6.7 Reinforced concrete cross-section for Example 6.3 (dimensions in mm).

Uncracked sections 241 of the coordinate system is taken at the centroid of the section (calculated based on instantaneous material properties) located at dx.ref = dy.ref = 215.6 mm, as shown in Fig. 6.7. The material behaviour is linear-elastic with Ec,0 = 32 GPa and Es = 200 GPa. The modular ratio for all reinforcement is therefore ns,0 = Es /Ec,0 = 6.25. Based on the adopted reference system, the coordinates of the steel reinforcement are: xs(1) = −155.6 mm; ys(1) = −155.6 mm xs(2) = 24.4 mm; ys(2) = −155.6 mm xs(3) = 204.4 mm; ys(3) = −155.6 mm xs(4) = −155.6 mm; ys(4) = 24.4 mm xs(5) = 24.4 mm; ys(5) = 24.4 mm xs(6) = 204.4 mm; ys(6) = 24.4 mm xs(7) = −155.6 mm; ys(7) = 204.4 mm xs(8) = 24.4 mm; ys(8) = 204.4 mm and the coordinates of the corners of the concrete section (numbered 1–6 in Fig. 6.7) are: x(1) = −215.6 mm; y(1) = −215.6 mm x(2) = 264.4 mm; y(2) = −215.6 mm x(3) = 264.4 mm; y(3) = 84.4 mm xs(4) = 84.4 mm; ys(4) = 84.4 mm xs(5) = 84.4 mm; ys(5) = 264.4 mm xs(6) = −215.6 mm; ys(6) = 264.4 mm The vectors of external loads and prestressing are: ⎡ ⎡ ⎤ ⎤ −800 × 103 N 0N re,0 = ⎣ 50 × 106 Nmm ⎦ and fp,init = ⎣ 0 Nmm ⎦ 0 Nmm 25 × 106 Nmm The properties of the transformed cross-section are: 8 0 A0 = bD − b2 D2 + (ns,0 − 1) As(i) = 216.9 × 103 mm2

i=1

D1 D2 Bx,0 = bD1 − dy.ref + b1 D2 D1 + − dy.ref 2 2 8 0 As(i) ys(i) = 0 mm3 + (ns,0 − 1) i=1

8 0 b b1 By,0 = bD1 − dx.ref + b1 D2 − dx.ref + (ns,0 − 1) As(i) xs(i) 2 2 i=1 = 0 mm3

2

2 bD31 b1 D32 D1 D2 Ix,0 = + bD1 + + b 1 D2 D 1 + + − dy.ref − dy.ref 12 12 2 2 8 0 2 = 3861 × 106 mm4 (ns,0 − 1) As(i) ys(i) i=1

242 Uncracked sections Iy,0 =

2

2 D2 b31 D1 b3 b b1 + bD1 − dx.ref + + b1 D2 − dx.ref 12 2 12 2 8 0 + (ns,0 − 1) As(i) x2s(i) = 3861 × 106 mm4 ; i=1

D1 b D2 Ixy,0 = bD1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref + (ns,0 − 1) As(i) xs(i) ys(i) = −934.3 × 106 mm4 . × 2 i=1 The fact that Bx,0 = By,0 = 0 could have also been concluded by noting that the origin of the coordinate system coincides with the centroid of the cross-section. Considering the ﬁrst moments of area about both axes are nil (i.e. Bx,0 = By,0 = 0), Eq. 6.29a simpliﬁes to: ⎡

⎤ 2 Ix,0 Iy,0 − Ixy,0 0 0 ⎣ F0 = 0 A0 Iy,0 A0 Ixy,0 ⎦ 2 A0 Ix,0 Iy,0 − Ixy,0 Ec,0 0 A0 Ixy,0 A0 Ix,0 1

⎡

⎤ 1.441 × 10−10 0 0 =⎣ 0 8.597 × 10−15 −2.080 × 10−15 ⎦ 0 −2.080 × 10−15 8.597 × 10−15 and ε0 is calculated using Eq. 6.18: ⎤ ⎡ −115.3 × 10−6 ε0 = F0 re,0 − fp,init = ⎣ 0.378 × 10−6 mm−1 ⎦ 0.111 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,0 = −115.3 × 10−6 κx,0 = 0.378 × 10−6 mm−1 κy,0 = 0.111 × 10−6 mm−1 The strains at the corners of the cross-section are obtained from Eq. 6.1: ε0(corner 1) = −172.8 × 10−6 ε0(corner 2) = −226.0 × 10−6 ε0(corner 3) = −112.6 × 10−6 ε0(corner 4) = −92.7 × 10−6 ε0(corner 5) = −24.6 × 10−6 ε0(corner 6) = 8.55 × 10−6

Uncracked sections 243 and the corresponding concrete stresses are obtained using Eq. 5.16a: σc,0(corner 1) = Ec,0 ε0(corner 1) = −5.53 MPa σc,0(corner 2) = −7.23 MPa σc,0(corner 3) = −3.60 MPa σc,0(corner 4) = −2.97 MPa σc,0(corner 5) = −0.79 MPa σc,0(corner 6) = 0.27 MPa The strains in the steel reinforcing bars are: εs(1),0 = −156.8 × 10−6 εs(2),0 = −176.8 × 10−6 εs(3),0 = −196.7 × 10−6 εs(4),0 = −88.8 × 10−6 εs(5),0 = −108.7 × 10−6 εs(6),0 = −128.7 × 10−6 εs(7),0 = −20.8 × 10−6 εs(8),0 = −40.7 × 10−6 and from Eq. 5.16b, the steel stresses are: σs(1),0 = −31.4 MPa σs(2),0 = −35.4 MPa σs(3),0 = −39.3 MPa σs(4),0 = −17.8 MPa σs(5),0 = −21.7 MPa σs(6),0 = −25.7 MPa σs(7),0 = −4.15 MPa σs(8),0 = −8.14 MPa The slope of the applied moment Me,0 is calculated based on Eq. 6.4: tan θM,0 =

Mye,0 25 × 106 = = 0.5 and therefore θM,0 = 26.56◦ Mxe,0 50 × 106

while the slope of the neutral axis is obtained using Eq. 6.22: tan θNA,0 =

κy,0 0.111 × 10−6 = = 0.293 and therefore θNA,0 = 16.31◦ . κx,0 0.378 × 10−6

The intersection of the neutral axis with the y-axis is calculated from Eq. 6.23: y(x = 0) = −

εr,0 −115.3 × 10−6 =− = +304.8 mm. κx,0 0.378 × 10−6

244 Uncracked sections The calculated stresses and strains are shown in Fig. 6.8. 16.31° −226.0 × 10−6 −7.23 x

−39.3 −35.4 −31.4

Me,0

−25.7 −21.7 Neutral axis

−17.8 y −8.14

e 8.55 × 10−6

−4.15 0.27

s

Figure 6.8 Initial strain and stress diagrams at time τ0 for Example 6.3 (all units in mm, MPa).

6.3 Long-term analysis using the age-adjusted effective modulus method (AEMM) The time analysis based on the AEMM to determine stresses and strains on a crosssection at time τk after a period of sustained loading was presented in Chapters 4 and 5 and only the steps relevant to the case of biaxial bending will be presented here. The constitutive relationships adopted for the concrete and steel are those already deﬁned for the AEMM in Eqs 5.22. With the instantaneous stress and strain distributions determined at time τ0 using the analysis of the previous section, the strain diagram at time τk is deﬁned by the strain at the origin and the curvatures about the orthogonal reference axes, i.e. εr,k , κx,k and κy,k . These are obtained by solving the equilibrium equations deﬁned by: re,k = ri,k

(6.33)

where T re,k = Ne,k Mxe,k Mye,k

(6.34a)

Uncracked sections 245 and T ri,k = Ni,k Mxi,k Myi,k

(6.34b)

Based on the material constitutive relationships (Eqs 5.22), the axial force resisted by each component of the cross-section at τk can be determined from: Nc,k = σc,k dA = Ee,k εr,k + yκx,k − xκy,k − εsh,k + Fe,0 σc,0 dA Ac

Ac

= Ac Ee,k εr,k + Bxc Ee,k κx,k − Byc Ee,k κy,k − Ac Ee,k εsh,k + Fe,0 Nc,0 Ns,k = RA,s εr,k + RBx,s κx,k − RBy,s κy,k Np,k = RA,p εr,k + RBx,p κx,k − RBy,p κy,k +

(6.35a) (6.35b)

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

i=1

(6.35c) These expressions can be summed to give the axial force resisted by the whole section Ni,k : Ni,k = RA,k εr,k + RBx,k κx,k − RBy,k κy,k − Ac Ee,k εsh,k + Fe,0 Nc,0 +

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36a)

i=1

and, in a similar manner, the internal moments about the x- and y-axes can be determined from: Mxi,k = RBx,k εr,k + RIx,k κx,k − RIxy,k κy,k − Bxc Ee,k εsh,k + Fe,0 Mxc,0 +

mp

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36b)

i=1

Myi,k = −RBy,k εr,k − RIxy,k κx,k + RIy,k κy,k + Byc Ee,k εsh,k + Fe,0 Myc,0 −

mp

xp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),k

(6.36c)

i=1

where the time-dependent cross-sectional rigidities at time τk are determined from expressions similar to those at time τ0 (Eqs 6.15) except that the age-adjusted effective modulus of the concrete Ee,k is used instead of the elastic modulus Ec,0 . That is: RA,k = Ac Ee,k + RA,s + RA,p

(6.37a)

RIxy,k = Ixyc Ee,k + RIxy,s + RIxy,p

(6.37b)

RBx,k = Bxc Ee,k + RBx,s + RBx,p

(6.37c)

246 Uncracked sections RBy,k = Byc Ee,k + RBy,s + RBy,p

(6.37d)

RIx,k = Ixc Ee,k + RIx,s + RIx,p

(6.37e)

RIy,k = Iyc Ee,k + RIy,s + RIy,p

(6.37f)

Substituting Eqs 6.36 into Eq. 6.33 produces the equilibrium equations describing the structural response at τk : re,k = Dk εk + fcr,k − fsh,k + fp,init − fp.rel,k where

⎤ εr,k εk = ⎣ κx,k ⎦ κy,k ⎡ ⎤ RA,k RBx,k −RBy,k Dk = ⎣ RBx,k RIx,k −RIxy,k ⎦ −RBy,k −RIxy,k RIy,k ⎡ ⎤ ⎡ ⎤ Ac εr,0 + Bxc κx,0 − Byc κy,0 Nc,0 ⎢ ⎥ fcr,k = Fe,0 ⎣ Mxc,0 ⎦ = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ Myc,0 −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 ⎤ ⎡ Ac ⎥ ⎢ fsh,k = ⎣ Bxc ⎦ Ee,k εsh,k −Byc

(6.38)

⎡

(6.39a)

(6.39b)

(6.39c)

(6.39d)

The variables describing the strain diagram at τ0 , i.e. εr,0 , κx,0 and κy,0 , are assumed to be known from the instantaneous analysis. The initial prestressing is included in f p,init (already deﬁned for the instantaneous analysis in Eq. 6.17d) and the steel relaxation is considered by means of f p.rel,k calculated as: ⎡ ⎤ mp A E p(i) p(i) ⎢ ⎥ (6.40) fp.rel,k = ⎣ yp(i) Ap(i) Ep(i) ⎦ εp(i),init ϕp (τk , σp(i),init ) i=1 −xp(i) Ap(i) Ep(i) Solving Eq. 6.38, the strain diagram at time τk is given by: εk = Fk re,k − fcr,k + fsh,k − fp,init + fp.rel,k

(6.41)

where ⎡

⎤ RBy,k RIxy,k −RBx,k RIy,k RBy,k RIx,k −RBx,k RIxy,k RIx,k RIy,k −R2Ixy,k 1 ⎢ RA,k RIy,k −R2By,k RA,k RIxy,k −RBx,k RBy,k ⎥ Fk = ⎣ RBy,k RIxy,k −RBx,k RIy,k ⎦ Rk RBy,k RIx,k −RBx,k RIxy,k RA,k RIxy,k −RBx,k RBy,k RA,k RIx,k −R2Bx,k

(6.42a)

Uncracked sections 247 and Rk = RA,k RIx,k RIy,k − R2Ixy,k − R2Bx,k RIy,k + 2RBx,k RBy,k RIxy,k − R2By,k RIx,k (6.42b) The stress distribution at time τk can then be calculated using equations similar to Eqs 5.41 as follows: & ' Ee,k εk − εsh,k + Fe,0 σc,0 = Fe,0 σc,0 Ee,k 1 y −x εk − εsh,k + σc,k = (6.43a) σs,k(i) = Es(i) εk = Es(i) 1 ys(i) − xs(i) εk (6.43b) σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k = Ep(i) 1 yp(i) − xp(i) εk + Ep(i) εp(i),init − Ep(i) εp.rel(i),k

(6.43c)

where at any point (x, y) on the cross-section εk = εr,k + yκx,k − xκy,k = 1 y −x εk . Similar to Eq. 6.21, the position of the neutral axis at time τk is given by: y=

κy,k κx,k

x−

εr,k κx,k

(6.44)

while its slope and its intersect with the y-axis may be calculated using: tan θNA,k =

κy,k

(6.45a)

κx,k εr,k y(x = 0) = − κx,k

(6.45b)

The expression for Fk can be signiﬁcantly simpliﬁed for doubly symmetric crosssections when the origin is located at the centroid of the section and the orthogonal axes are parallel to the axes of symmetry. In this case, RIxy,k = RBx,k = RBy,k = 0 and Fk is given by: ⎡

⎤ RIx,k RIy,k 0 0 1 ⎢ ⎥ 0 RA,k RIy,k 0 Fk = ⎣ ⎦ RA,k RIx,k RIy,k 0 0 RA,k RIx,k

(6.46)

As discussed previously for the instantaneous analysis, the cross-sectional rigidities included in Fk can be calculated based on the properties of the age-adjusted transformed cross-section. For this purpose, modular ratios of n¯ s(i),k = Es(i) / Ee,k and n¯ p(i),k = Ep(i) / Ee,k are to be used for the i-th steel bar and the i-th tendon, respectively.

248 Uncracked sections

Example 6.4 For the reinforced concrete section and coordinate system of Example 6.2 (Fig. 6.5), if the external actions (i.e. Ne = −500 kN, Mxe = 25 kNm, Mye = 25 kNm) are sustained over a period of time (τ0 to τk ), the longterm effects caused by creep and shrinkage are to be determined. As for Example 6.2, Ec,0 = 32 GPa, Es = 200 GPa, and ns,0 = Es /Ec,0 = 6.25. The creep coefﬁcient, the ageing coefﬁcient and the shrinkage strain associated with the time period under consideration are ϕ(τk , τ0 ) = 2.0; χ(τk , τ0 ) = 0.65 and εsh (τk ) = −400 × 10−6 . From Example 6.2 at τ0 : εr,0 = −116.4 × 10−6 ; κx0 = 0.431 × 10−6 mm−1 ; κy0 = 0.770 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 32,000 = 13,910 MPa = 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.0 and therefore n¯ s,k = 14.38

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.0 × (0.65 − 1.0) Fe,0 = = −0.304 = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.0 For this reinforced concrete section, the vectors re,k , fp,init and fp.rel,k in Eq. 6.41 are: ⎡ ⎤ −500 × 103 N ⎢ ⎥ re,k = ⎣ 25 × 106 Nmm ⎦ 25 × 106 Nmm ⎡ ⎤ 0N ⎢ ⎥ fp,init = ⎣ 0 Nmm ⎦ 0 Nmm ⎡ ⎤ 0N ⎢ ⎥ fp.rel,k = ⎣ 0 Nmm ⎦ 0 Nmm The properties of the age-adjusted transformed cross-section based on Ee,k are: 6 0 ¯ k = bD + (n¯ s,k − 1) As(i) = 156.1 × 103 mm2 A

2 i=1 3 6 0 bD D 2 = 2141 × 106 mm4 I¯x,k = + bD − dy.ref + (n¯ s,k − 1) As(i) ys(i) 12 2 i=1

2 6 0 Db3 b I¯y,k = + bD − dx.ref + (n¯ s,k − 1) As(i) x2s(i) = 1192 × 106 mm4 12 2 i=1 B¯ x,k = B¯ y,k = I¯xy,k = 0

Uncracked sections 249 The geometric properties of the concrete are required for the calculation of f cr,k and f sh,k and are obtained as follows: Ac = bD −

6 0

As(i) = 117.3 × 103 mm2

2 6 0 bD3 D 2 = 1559 × 106 mm4 Ixc = + bD − dy.ref − As(i) ys(i) 12 2 i=1

2 6 0 Db3 b Iyc = + bD As(i) x2s(i) = 878.1 × 106 mm4 − dx.ref − 12 2 i=1 Bxc = Byc = Ixyc = 0 i=1

From Eqs 6.39c and d: ⎡

⎤ ⎡ ⎤ 133.0 × 103 N Ac εr,0 + Bxc κx,0 − Byc κy,0 fcr,k = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ = ⎣ −6.55 × 106 Nmm ⎦ −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 −6.58 × 106 Nmm ⎤ ⎤ ⎡ ⎡ 117.3 × 103 −652.8 × 103 N −6 ⎦ ⎦ × 13,910 × −400 × 10 =⎣ fsh,k = ⎣ 0 Nmm 0 0 Nmm 0 Based on properties of the age-adjusted transformed cross-section, Fk is calculated using Eq. 6.46 as: ⎡

⎤ 4.604×10−10 N−1 0 0 ⎢ ⎥ Fk = ⎣ 0 3.356×10−14 N−1 mm−2 0 ⎦ −1 −14 −2 0 0 6.027 ×10 N mm

The strain εk at time τk is obtained using Eq. 6.41: ⎤ ⎡ −592.0 × 10−6 εk = Fk (re,k − fcr,k + fsh,k ) = ⎣ 1.058 × 10−6 mm−1 ⎦ 1.903 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,k = −592.0 × 10−6 κx,k = 1.058 × 10−6 mm−1 κy,k = 1.903 × 10−6 mm−1 The strains at the corners of the cross-section are (Eq. 6.1): εk(top-left) (x = −b/2, y = −D/2) = −518.2 × 10−6 εk(top-right) (x = b/2, y = −D/2) = −1089 × 10−6 εk(btm-right) (x = b/2, y = D/2) = −665.8 × 10−6 εk(btm-left) (x = −b/2, y = D/2) = −94.7 × 10−6

250 Uncracked sections The stresses in the concrete and in the steel reinforcement are calculated using Eqs 5.16: & ' σc,k(top-left) = Fe,0 σc,0(top-left) Ee,k 1 yc,(top-left) −xc,(top-left) εk − εsh,k + ⎧ ⎫ ⎡ ⎤ −6 ⎨ ⎬ −592.0 × 10−6 ⎦ − −400 × 10−6 = 13,910 × 1 −200 −(−150) ⎣ 1.058 × 10 ⎩ ⎭ 1.903 × 10−6 + (−0.304) (−2.79) = −0.79 MPa σc,k(top-right) = −6.49 MPa σc,k(btm-right) = −2.28 MPa σc,k(btm-left) = 3.42 MPa σs(1),k = Es 1 ys(1) −xs(1) εk

⎤ −592.0 × 10−6 = 200 × 103 × 1 −150 −(−90) × ⎣ 1.058 × 10−6 ⎦ 1.903 × 10−6 = −115.9 MPa; σs(2),k = −184.4 MPa σs(3),k = −84.1 MPa σs(4),k = −152.7 MPa σs(5),k = −52.4 MPa σs(6),k = −120.8 MPa

⎡

Stresses and strains calculated at time τk are shown in Fig. 6.9. Signiﬁcant transfer of axial compressive load took place from the concrete to the steel with time, with the maximum compressive stress in the concrete reducing from −10.18 MPa at τ0 to −6.49 MPa at τk and the compressive stress in the most heavily stressed reinforcing bar increasing from −50.1 MPa to −184.4 MPa. It is also noted that the tensile stress in the concrete in the bottom left corner of the cross-section has increased from 2.73 MPa to 3.42 MPa, indicating that cracking may well occur during a period of sustained loading (primarily due to shrinkage). The slopes of the applied moment Me,k and the neutral axis are (Eqs 6.4 and 6.45a): tan θM,k = tan θM,0 = 1.0 and therefore θM,k = 45◦ and tan θNA,k =

κy,k κx,k

=

1.903 × 10−6 = 1.80 and therefore θNA,k = 60.91◦ . 1.058 × 10−6

The neutral axis passes through the y-axis at (Eq. 6.45b): y=−

εr,k −592.0 × 10−6 =− = 559.2 mm κx,k 1.058 × 10−6

This indicates a translation of the neutral axis with a slight rotation from the results previously obtained at time τ0 . In fact, the slope of the neutral axis varies

Uncracked sections 251

60.91°

x 45° −1089.3 × 10−6

Me,k

y Neutral axis −184.4 −6

−94.7 × 10

−152.7 −120.9 −115.9

e

−6.49

−84.1 −52.4

σ

3.42

Figure 6.9 Final strain and stress diagrams at time τk (Example 6.4) (all units in mm, MPa).

from θNA,0 = 60.76◦ to θNA,k = 60.91◦ while the intersection with the y-axis moves from y = 270.2 mm at τ0 to y = 559.2 mm at τk . The translation of the neutral axis is mostly due to the effects of shrinkage. If the example was repeated with shrinkage set to zero, the intersection with the y-axis would change only slightly from y = 270.2 mm at τ0 to y = 275.3 mm at τk .

Example 6.5 The long-term strains and stresses on the cross-section of Fig. 6.7 are to be determined using the AEMM assuming that the external loads applied in Example 6.3 (i.e. Ne = −800 kN, Mxe = 50 kNm, Mye = 25 kNm) are to be

252 Uncracked sections sustained between times τ0 and τk . The instantaneous material properties are the same as in Example 6.3: Ec,0 = 32 GPa, Es = 200 GPa, and ns,0 = Es /Ec,0 = 6.25. The creep coefﬁcient, ageing coefﬁcient and shrinkage strain associated with the time period τ0 to τk are: ϕ(τk , τ0 ) = 2.0; χ (τk , τ0 ) = 0.65 and εsh (τk ) = − 400 × 10−6 . From Example 6.3 at τ0 : εr,0 = −115.3 × 10−6 ; κx0 = 0.378 × 10−6 mm−1 ; κy0 = 0.111 × 10−6 mm−1 . From Eqs 4.35 and 4.46: Ee,k =

Ec,0 32,000 = = 13,910 MPa 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 2.0 and therefore n¯ s,k = 14.38

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 2.0 × (0.65 − 1.0) Fe,0 = = −0.304 = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 2.0 and for this reinforced concrete section, the vectors re,k , fp,init and fp.rel,k in Eq. 6.41 are: ⎡ ⎤ −800 × 103 N re,k = ⎣ 50 × 106 Nmm ⎦ 25 × 106 Nmm ⎡ ⎤ 0N fp,init = ⎣ 0 Nmm ⎦ 0 Nmm ⎡ ⎤ 0N fp.rel,k = ⎣ 0 Nmm ⎦ 0 Nmm The properties of the age-adjusted transformed cross-section based on Ee,k are: ¯ k = bD − b2 D2 + (n¯ s,k − 1) A

8 0

As(i) = 246.2 × 103 mm2

i=1

D1 D2 B¯ x,k = bD1 − dy.ref + b1 D2 D1 + − dy.ref 2 2 8 0 As(i) ys(i) = 62.69 × 103 mm3 + (n¯ s,k − 1)

i=1

8 0 b b1 B¯ y,k = bD1 As(i) xs(i) − dx.ref + b1 D2 − dx.ref + (n¯ s,k − 1) 2 2 i=1 = 62.69 × 103 mm3

2

2 bD31 b1 D32 D1 D2 ¯Ix,k = − dy.ref + − dy.ref + bD1 + b1 D2 D1 + 2 2 12 12 8 0 2 = 4439 × 106 mm4 + (n¯ s,k − 1) As(i) ys(i) i=1

2

D2 b31 D1 b3 b I¯y,k = + bD1 − dx.ref + + b1 D2 12 2 12 8 0 + (n¯ s,k − 1) As(i) x2s(i) = 4439 × 106 mm4

Uncracked sections 253

2 b1 − dx.ref 2

i=1

b D2 ¯Ixy,k = bD1 D1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref + (n¯ s,k − 1) As(i) xs(i) ys(i) = −1067 × 106 mm4 × 2 i=1 The geometric properties of the concrete are required to evaluate f cr,k and f sh,k : Ac = bD − b2 D2 − Bxc = bD1

8 0

As(i) = 194.4 × 103 mm2

i=1

D1 − dy.ref 2

8 0 D2 + b1 D2 D1 + As(i) ys(i) − dy.ref − 2 i=1

= −35.64 × 103 mm3

8 0 b b1 Byc = bD1 − dx.ref + b1 D2 − dx.ref − As(i) xs(i) 2 2 i=1 = −35.64 × 103 mm3

2

2 bD31 b1 D32 D1 D2 Ixc = + bD1 − dy.ref + + b1 D2 D1 + − dy.ref 12 2 12 2 −

8 0 i=1

Iyc =

2 = 3417 × 106 mm4 As(i) ys(i)

2

2 D2 b31 b b1 D1 b3 + bD1 − dx.ref + + b1 D2 − dx.ref 12 2 12 2 −

8 0 i=1

As(i) x2s(i) = 3417 × 106 mm4

D1 b D2 Ixyc = bD1 − dy.ref − dx.ref + b1 D2 D1 + − dy.ref 2 2 2

8 0 b1 − dx.ref − As(i) xs(i) ys(i) = −831.9 × 106 mm4 × 2 i=1 From Eqs 6.39c and d: ⎡

⎤

⎡

⎤ 218.3 × 103 N ⎢ ⎥ ⎢ ⎥ fcr,k = Fe,0 Ec,0 ⎣ Bxc εr,0 + Ixc κx,0 − Ixyc κy,0 ⎦ = ⎣ −13.52 × 106 Nmm ⎦ −6.705 × 106 Nmm −Byc εr,0 − Ixyc κx,0 + Iyc κy,0 Ac εr,0 + Bxc κx,0 − Byc κy,0

254 Uncracked sections ⎡

⎤ ⎡ ⎤ 194.4 × 103 Ac fsh,k = ⎣ Bxc ⎦ Ee,k εsh,k = ⎣ −35.64 × 103 ⎦ × 13,910 × −400 × 10−6 −Byc 35.64 × 103 ⎡ ⎤ −1082 × 103 N = ⎣ 0.198 × 106 Nmm ⎦ −0.198 × 106 Nmm Based on properties of the age-adjusted transformed cross-section, Fk is calculated using Eq. 6.42a, except that the age-adjusted modulus Ee,k is used instead of Ec,0 : ⎡

2.920×10−10

⎢ Fk = ⎣ −5.429×10−15 5.429×10−15

−5.429×10−15 1.719×10−14 −4.133×10−15

5.429×10−15

⎤

⎥ −4.133×10−15 ⎦ 1.719×10−14

The strain εk at time τk is obtained using Eq. 6.41: ⎡

⎤ −613.4 × 10−6 εk = Fk (re,k − fcr,k + fsh,k ) = ⎣ 0.976 × 10−6 mm−1 ⎦ 0.267 × 10−6 mm−1 The strain at the origin and the curvatures with respect to the x- and y-axes, respectively, are: εr,k = −613.4 × 10−6 κx,k = 0.976 × 10−6 mm−1 κy,k = 0.267 × 10−6 mm−1 The strains at the corners of the cross-section are obtained from Eq. 6.1: εk(corner 1) = −766.4 × 10−6 εk(corner 2) = −894.4 × 10−6 εk(corner 3) = −601.6 × 10−6 εk(corner 4) = −553.5 × 10−6 εk(corner 5) = −377.8 × 10−6 εk(corner 6) = −297.8 × 10−6 and the corresponding concrete stresses are obtained using Eq. 6.43a: ' 1 ycorner 1 −xcorner 1 εk − εsh,k + Fe,0 σc,0(corner 1) = −3.41 MPa σc,k(corner 2) = −4.68 MPa σc,k(corner 3) = −1.71 MPa

σc,k(corner 1) = Ee,k

&

Uncracked sections 255 σc,k(corner 4) = −1.23 MPa σc,k(corner 5) = 0.55 MPa σc,k(corner 6) = 1.34 MPa The strains in the steel reinforcing bars are: εs(1),k = −723.8 × 10−6 εs(2),k = −771.9 × 10−6 εs(3),k = −819.9 × 10−6 εs(4),k = −548.1 × 10−6 εs(5),k = −596.1 × 10−6 εs(6),k = −644.1 × 10−6 εs(7),k = −372.4 × 10−6 εs(8),k = −420.4 × 10−6 and from Eq. 6.43b, the steel stresses are: σs(1),k = −144.8 MPa σs(2),k = −154.4 MPa σs(3),k = −164.0 MPa σs(4),k = −109.6 MPa σs(5),k = −119.2 MPa σs(6),k = −128.8 MPa σs(7),k = −74.5 MPa σs(8),k = −84.1 MPa The slope of the applied moment Me,k is calculated based on Eq. 6.4 at time τk : tan θM,k =

Mye,k Mxe,k

=

25 × 106 = 0.5 and therefore θM,k = 26.56◦ 50 × 106

The equation of the line of the neutral axis at time τk (in the x-y plane) is from Eq. 6.44: y=

κy,k κx,k

x−

εr,k 0.267 × 10−6 −613.4 × 10−6 = x − = 0.273x + 628.3 κx,k 0.976 × 10−6 0.976 × 10−6

and with tan θNA,k = 0.273, the inclination of the neutral axis is θNA,k = 15.28◦ and it passes through the y-axis at y = 628.3 mm. Without shrinkage, the intersection with the y-axis occurs at y(x = 0) = 307.9 mm (close to the value of 304.8 mm calculated at time τ0 ).

256 Uncracked sections The ﬁnal stresses and strains on the cross-section are shown in Fig. 6.10. 15.28° −894.4 × 10−6 −4.68

−164.0 −154.4

x

−144.8 Me,k

26.56°

−128.8 −119.2 −109.6

−84.1

y −297.8 × 10−6

−74.5 e

1.34

s

Figure 6.10 Final strain and stress diagrams at time τk for Example 6.5 (all units in mm, MPa).

6.4 Long-term analysis using the step-by-step method The use of the SSM is particularly useful for the long-term analysis of reinforced concrete columns as it enables complex loading histories to be considered, such as those that occur during different construction stages. It also permits improved accuracy with ﬁner time discretisation. In the following, only the steps peculiar to combined axial force and biaxial moments are presented as the use of the SSM has been extensively discussed in Chapters 4 and 5. When using the SSM the time domain is discretised into a number of instants τj , with j = 1, . . ., k and with τk being the instant at which the long-term response is sought. The constitutive relationships for the concrete and the steel reinforcement and tendons are deﬁned in Eqs 4.25 and 5.44. The solution process is similar to that already outlined for both the instantaneous analysis and time analysis using the AEMM. At any time instant τj , the problem is expressed in terms of the three variables that deﬁne the strain diagram (εr,j , κx,j and κy,j ) and these are determined based on equilibrium considerations written as: re,j = ri,j

(6.47)

Uncracked sections 257 where re,j and ri,j represent the external and internal actions, and similarly to Eq. 5.46, may be expressed by: T re,j = Ne,j Mxe,j Mye,j

(6.48a)

T ri,j = Ni,j Mxi,j Myi,j

(6.48b)

and

The internal actions ri,j are expressed in terms of the strain measured at the origin of the reference system (εr,j ), and the curvatures calculated with respect to the x- and y-axes (κx,j and κy,j ). Using the constitutive relationships speciﬁed in Eqs 4.25 and 5.44, the contribution to the internal axial force carried by the concrete, the steel reinforcement and the tendons at time τj may be written as:

Nc,j =

σc,j dA = Ac

⎡

⎤ j−1 ⎣Ec,j εr,j + yκx,j − xκy,j − εsh,j + Fe,j,i σc,i ⎦ dA i=0

Ac

= Ac Ec,j εr,j + Bxc Ec,j κx,j − Byc Ec,j κy,j − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

(6.49a)

i=0

Ns,j = RA,s εr,j + RBx,s κx,j − RBy,s κy,j Np,j = RA,p εr,j + RBx,p κx,j − RBy,p κy,j +

(6.49b) mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.49c)

i=1

where the cross-sectional rigidities have been introduced previously in Eqs 6.7, 6.10 and 6.13. The expression for Ni,j (included in ri,j ) can be obtained by summing Eqs 6.49: Ni,j = RA,j εr,j + RBx,j κx,j − RBy,j κy,j − Ac Ec,j εsh,j +

j−1

Fe,j,i Nc,i

i=0

+

mp

Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50a)

i=1

Similarly, the expressions for the internal moments are given by: Mxi,j = RBx,j εr,j + RIx,j κx,j − RIxy,j κy,j − Bxc Ec,j εsh,j +

j−1

Fe,j,i Mxc,i

i=0

+

mp i=1

yp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50b)

258 Uncracked sections Myi,j = −RBy,j εr,j − RIxy,j κx,j + RIy,j κy,j + Byc Ec,j εsh,j +

j−1

Fe,j,i Myc,i

i=0 mp

−

xp(i) Ap(i) Ep(i) εp(i),init − εp.rel(i),j

(6.50c)

i=1

where the cross-sectional rigidities are determined using Eqs 6.15 (proposed for the instantaneous analysis) except that the concrete elastic modulus at time τj , Ec,j , is used instead of the instantaneous value at time τ0 , Ec,0 . The equilibrium equations of Eqs 6.47 can be expressed in compact form at time τj as: re,j = Dj εj + fcr,j − fsh,j + fp,init − fp.rel,j

(6.51)

where: ⎡

⎤ εr,j εj = ⎣ κx,j ⎦ κy,j ⎡ ⎤ RBx,j −RBy,j RA,j RIx,j −RIxy,j ⎦ Dj = ⎣ RBx,j −RBy,j −RIxy,j RIy,j fcr,j =

j−1

Fe,j,i rc,i

(6.52a)

(6.52b)

(6.52c)

i=0

⎡

⎤ Ac fsh,j = ⎣ Bxc ⎦ Ec,j εsh,j −Byc ⎡ ⎤ mp Ap(i) Ep(i) εp(i),init ⎢ ⎥ fp,init = ⎣ yp(i) Ap(i) Ep(i) εp(i),init ⎦ i=1 −xp(i) Ap(i) Ep(i) εp(i),init ⎡ ⎤ mp Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) ⎢ ⎥ fp.rel,j = ⎣ yp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init ) ⎦ i=1 −xp(i) Ap(i) Ep(i) εp(i),init ϕp (τj , σp(i),init )

(6.52d)

(6.52e)

(6.52f)

where rc,i included in the calculation of f cr,j depicts the internal actions resisted by the concrete part of the cross-section at time τi (for which i < j) and is calculated based on: ⎡

⎤ ⎡ ⎤ i−1 Nc,i Ac rc,i = ⎣ Mxc,i ⎦ = Dc,i εi + Fe,i,n rc,n − ⎣ Bxc ⎦ Ec,i εsh,i = Dc,i εi + fcr,i − fsh,i Myc,i −Byc n=0 (6.53)

Uncracked sections 259 in which ⎤ Ac Bxc −Byc ⎥ ⎢ Dc,i = ⎣ Bxc Ixc −Ixyc ⎦ Ec,i −Byc −Ixyc Iyc ⎡

(6.54)

The strain diagram at time τj can then be determined based on: εj = Fj re,j − fcr,j + fsh,j − fp,init + fp.rel,j

(6.55)

in which Fj is identical to F0 (deﬁned in Eqs 6.19), except that concrete elastic modulus Ec,j replaces Ec,0 . The stress distribution at time τk can then be calculated substituting the expression for the strain εk = εr,k + yκx,k − xκy,k = 1 y −x εk into Eqs 5.60. The simpliﬁcations proposed for doubly-symmetric columns previously introduced for the instantaneous analysis and for the time analysis using the AEMM, can also be applied at time τj when using the SSM. As in the previous analyses, the cross-sectional rigidities included in Fj could be calculated based on the transformed concrete cross-section obtained using the appropriate modular ratios ns(i),j = Es(i) /Ec,j and np(i),j = Ep(i) /Ec,j for the i-th steel bar and the i-th tendon, respectively.

7

Cracked sections

7.1 Introductory remarks In the cross-sectional analyses of Chapters 4, 5 and 6, it was assumed that concrete can carry imposed stresses, both compressive and tensile. However, in reality concrete is not able to carry large tensile stress. If the tensile stress at a point reaches the tensile strength of concrete (Eq. 2.1), cracking occurs. Cracking is irreversible. On a cracked cross-section, tensile stress of any magnitude cannot be carried normal to the crack surface at any time after cracking and tensile forces can only be carried across a crack by steel reinforcement. Therefore, on a cracked cross-section, internal actions can be carried only by the steel reinforcement (and tendons) and the uncracked parts of the concrete section. In members subjected only to axial tension, caused either by external loads or by restraint to shrinkage or temperature change, full-depth cracks occur when the tensile stress is exceeded (i.e. at each crack location, the entire cross-section is cracked). When the axial tension is caused by restraint to shrinkage, cracking causes a loss of stiffness and a consequent decrease in the internal tension. The crack width and the magnitude of the restraining force, as well as the spacing between the cracks, depend on the amount of bonded reinforcement. Between the cracks in a member subjected to axial tension, the concrete continues to carry tensile stress and hence continues to contribute to the member stiffness. This is the tension stiffening effect and was discussed in Section 3.6.2. When cracking occurs in ﬂexural members and the tensile strength of the concrete on the tensile surface of the member is reached, primary cracks develop at regular spacing on the tensile side of the member, as shown in Fig. 3.4a. A sudden loss of stiffness occurs at ﬁrst cracking and the short-term moment–curvature relationship becomes nonlinear. The primary cracks penetrate spontaneously to a height ho (see Fig. 3.4a) which depends on the quantity of steel and the magnitude of any axial force or prestress. For reinforced concrete members in pure bending with no axial force, the height of the primary cracks ho immediately after cracking is usually relatively high (0.6 to 0.9 times the depth of the member) and remains approximately constant under increasing bending moments until either the steel reinforcement yields or the concrete stress–strain relationship in the compressive region becomes non-linear. For prestressed members and members subjected to bending plus axial compression, ho may be relatively small initially and gradually increases as the applied moment increases, even when material behaviour is linear-elastic.

Cracked sections 261 The stress in the tensile reinforcement and the stress in the concrete at the steel level for the cracked member of Fig. 3.4a are illustrated in Figs 3.4b and c, respectively. Immediately after ﬁrst cracking, the intact concrete between adjacent primary cracks carries considerable tensile force, mainly in the direction of the reinforcement, due to the bond between the steel and the concrete. The average tensile stress in the concrete is a signiﬁcant percentage of the tensile strength of concrete. The steel stress is a maximum at a crack, where the steel carries the entire tensile force, and drops to a minimum between the cracks, as shown (Fig. 3.4b). The bending stiffness of the member is considerably greater than that based on a fully-cracked section, where concrete in tension is assumed to carry zero stress. This tension stiffening effect may be signiﬁcant in the service-load performance of beams and even more so for lightly reinforced slabs. The Euler–Bernoulli assumption that plane sections remain plane is not strictly true for a cross-section in the cracked region of a beam. However, if strains are measured over a gauge length containing several primary cracks, the average strain diagram is linear over the depth of the member. As the load increases above the cracking moment Mcr , and after the primary cracks have developed, secondary cracks (or cover-controlled cracks) form around the reinforcement between the primary cracks, the average concrete tensile stress drops and the tension stiffening effect gradually reduces. A typical moment versus average curvature relationship for a reinforced concrete cross-section in pure bending is shown in Fig. 7.1a as the solid line OAB in which Ms represents the applied service moment. Also shown as the dashed line OC of slope (EI)cr is the moment–curvature relationship for a fully-cracked cross-section. As moment increases after ﬁrst cracking, the ﬂexural rigidity gradually reduces from that of the uncracked section (EI)uncr at ﬁrst cracking and approaches that of the fully-cracked section, (EI)cr , as the moment becomes large, as shown. If an uncracked singly reinforced member such as that shown in Fig. 1.14a begins to shrink prior to loading, as is commonly the case, shrinkage warping occurs and a shrinkage-induced curvature κsh.uncr develops on the uncracked cross-section when the applied moment is still zero (i.e. Ms = 0) as shown in Fig. 7.1b as point O . The curvature κsh.uncr and the tensile stress caused by shrinkage in the extreme ﬁbre of the uncracked cross-section σcs were illustrated in Fig. 1.14b. Because of the initial tensile stress σcs in the concrete, the moment required to cause ﬁrst cracking Mcr.sh0 will be less than Mcr (as indicated in Fig. 7.1) and the moment-curvature relationship is now represented by curve O A B in Fig. 7.1b. The initial curvature due to early shrinkage on a fully-cracked cross-section (κsh.cr ) where the concrete is assumed to carry no tension is signiﬁcantly larger that that of the uncracked member (κsh.uncr ), as illustrated in Fig. 1.14. Therefore, early shrinkage before loading causes the dashed line representing the fully-cracked response to move further to the right, shown as line O C in Fig. 7.1b. For a prestressed concrete member, or a reinforced concrete member in combined bending and compression, the effect of tension stiffening is less pronounced because the loss of stiffness of the cracked section is less dramatic. As the applied moment increases, the depth of the primary cracks increases gradually (in contrast to the sudden crack propagation in a reinforced member in pure bending) and the depth of the concrete compressive zone is signiﬁcantly greater than would be the case if no axial force was present. A typical short-term moment-average curvature relationship for a

262 Cracked sections Tension stiffening, dk Moment

B Average M vs k

C

(EI )cr

(EI)uncr

Concrete carries no tension anywhere

Ms A

Mcr

Uncracked cross-section Curvature, k

O

(a) No shrinkage prior to loading B′ C′

Tension stiffening, dk

Moment

Average M vs k (EI )cr

(EI )uncr Ms

Concrete carries no tension anywhere

A′

Mcr.sh0

Uncracked cross-section O′ O ksh.uncr

O″ Curvature, k ksh.cr (b) Shrinkage strain esh,0 prior to loading

Figure 7.1 Moment-average curvature relationship for a reinforced concrete cross-section at ﬁrst loading, τ0 .

prestressed concrete cross-section containing bonded tensile reinforcement is shown in Fig. 7.2, together with the moment–curvature relationship for the cross-section containing a crack. The internal moment caused by the resultant prestressing force about the centroidal axis of the uncracked section is designated Pe. As can be seen by comparing the curves in Figs 7.1a and 7.2, the presence of the axial prestress signiﬁcantly changes the shape of curve after cracking. The prestressing force (or axial compression) increases the post-cracking stiffness and greatly improves the in-service behaviour of a concrete member after the onset of ﬂexural cracking. In Section 3.6.3, modular ratio theory was presented for the determination of the stresses and deformations of a singly-reinforced rectangular cross-section in pure

Cracked sections 263 M − Pe

Average M vs k

Concrete carries no tension anywhere

Slope of tangent = (EI)cr

M

Mcr

(EI)uncr Curvature, k

−Pe

Figure 7.2 Short-term moment-average curvature relationship for a prestressed concrete cross-section.

bending at a primary crack location. The properties of the fully-cracked cross-section, including the depth to the neutral axis kd (Eq. 3.14) and the second moment of area of the cracked section about its centroidal axis Icr (Eq. 3.17) were also derived. For a more general cross-section, the properties of the cracked section may be determined from a transformed section analysis in which the tensile concrete is ignored. Such an analysis is presented in Section 7.2. Cracking also inﬂuences the time-dependent behaviour of reinforced and prestressed concrete members. In Section 1.2.7, the effects of creep on a fully-cracked cross-section were compared with the corresponding effects on an uncracked cross-section (see Fig. 1.12), while the stresses and deformations caused by shrinkage on a cracked section were discussed in Section 1.3.3 and illustrated in Fig. 1.14b. For a cross-section subjected to constant sustained moment over the time period τ0 to t, if no shrinkage has occurred prior to loading, the instantaneous moment versus curvature response of the cross-section is shown as curve OAB in Fig. 7.3a (identical to curve OAB in Fig. 7.1a). The instantaneous fully-cracked section response (calculated ignoring the tensile concrete) is shown as dashed line OC in Fig. 7.3a. If the crosssection does not shrink with time (i.e. εsh remains at zero), creep causes an increase in curvature with time at all moment levels and the time-dependent M − κ response shifts to curve OA B in Fig. 7.3a. The creep-induced increase in curvature with time may be expressed as κcr (t) = κi ϕ(t, τ0 )/α, where κi is the instantaneous curvature, ϕ(t, τ0 ) is the creep coefﬁcient and α is a factor that depends on the amount of cracking and the reinforcement quantity and location. Approximate expressions for α were given in Eqs 3.32 and, for typical reinforcement ratios for beams and slabs, α is in the range 1.0– 1.3 prior to cracking and in the range 4–6 when cracking is extensive. With regard to the response of a fully-cracked cross-section (calculated ignoring the tensile concrete), creep causes a softening of the response shown as dashed line OC in Fig. 7.3a, with the slope of the line decreasing by the factor 1/(1 + ϕ(t, τ0 )/α), where α is in the range 4–6 depending on the reinforcement ratio.

264 Cracked sections Moment

B

B′

C

C′

Instantaneous member response D

M1

D′

E

A

Mcr

E′

Member response after creep at time t

A′

Fully-cracked response after creep at time t Instantaneous response of fullycracked section Curvature, k O

ki + Δk cr(t)

ki

(a) Effects of creep (zero shrinkage)

B

Moment

B′ C′

C

Instantaneous member response D

M1

D′

E

E′

A

Mcr

Member response after creep and shrinkage at time t

A′

Mcr.sh

Fully-cracked response after creep and shrinkage at time t Curvature, k O

O′

O″

ki

ki + Δkcr(t) + Δksh(t)

(b) Effects of creep and shrinkage

Figure 7.3 Moment-average curvature relationship for a reinforced concrete cross-section under sustained loads at time t.

When shrinkage before and after ﬁrst loading is included, the curvature increases even further with time and the time-dependent response of the cross-section is shown as curve O A B in Fig. 7.3b. At M = 0, the curvature increases due to shrinkage of the uncracked cross-section and the point O moves horizontally to O . Due to the restraint to shrinkage provided by the bonded reinforcement, tensile stress is induced with time and this has the effect of lowering the cracking moment from Mcr to Mcr.sh , as shown in Fig. 7.3b. For any cross-section subjected to a sustained moment in the range Mcr.sh < M ≤ Mcr , cracking will occur with time and the increase in curvature will be exacerbated by the loss of stiffness caused by time-dependent cracking. In practice, critical sections of many lightly reinforced slabs are loaded in this range.

Cracked sections 265 The response of the cracked section (ignoring the tensile concrete) after creep and shrinkage is shown as line O C in Fig. 7.3b. The shrinkage-induced curvature of the fully-cracked cross-section when M = 0 is greater than that of the uncracked crosssection and the cracked section response is shifted horizontally from point O to point O , as shown. The slope of the cracked section response in Fig. 7.3b is softened by creep and the slope of the line O C in Fig. 7.3b is the same as the slope of line OC in Fig. 7.3a. At a typical in-service moment M1 , the instantaneous curvature due to tension stiffening κ ts.0 is DE in Fig. 7.3b and the time-dependent tension stiffening curvature after the period of sustained loadings κ ts (t) is D E in Fig. 7.3b. Tension stiffening reduces under sustained loading, primarily due to time-dependent cracking, shrinkageinduced degradation of bond at the concrete-reinforcement interface and tensile creep between the cracks in the tensile concrete. It is generally believed that tension stiffening reduces rapidly after ﬁrst loading and reduces to about half its instantaneous value with time (Refs 1–4). When a fully-cracked cross-section is subjected to a period of sustained loading, creep causes a change in position of the neutral axis. In general, the depth to the neutral axis increases with time and, hence, so too does the area of concrete in compression. To account accurately for this gradual change of the properties of the cross-section, an iterative numerical solution procedure is required, in which the time period is divided into small increments and the cross-sectional properties at the end of each time increment are modiﬁed. While such a procedure is routinely implemented in ﬁniteelement models of cracked reinforced concrete, often using a layered cross-section, it is not suitable for manual solution. The time analysis of a cracked cross-section using the age-adjusted effective modulus method is presented in Section 7.3. In this analysis, the dimensions of the fully-cracked cross-section are assumed to remain constant throughout the time analysis, i.e. the depth of the concrete in compression and the extent of cracking are assumed to remain constant with time. This assumption is in fact necessary, if the short-term and time-dependent stress and strain increments are to be calculated separately and added together to obtain ﬁnal stresses and deformations, i.e. if the principle of superposition is to be applied to fully-cracked sections in the same way as it has been applied to uncracked cross-sections. The assumption also greatly simpliﬁes the analysis and usually results in relatively little error in the estimation of time-dependent deformations.

7.2 Short-term analysis In this section, the short-term responses of fully-cracked reinforced and partiallyprestressed concrete cross-sections subjected to combined bending and axial force are considered. The time-dependent effects of creep and shrinkage are considered in Section 7.3. As for the analyses of uncracked cross-sections in Chapters 4, 5 and 6, the analysis presented here is based on the following assumptions: • •

Plane sections remain plane and, as a consequence, the strain distribution is linear over the depth of the section. Perfect bond exists between the steel and the concrete, i.e. steel and concrete strains are assumed to be compatible. This is usually a reasonable assumption at service loads in members containing deformed steel reinforcing bars and strands.

266 Cracked sections • •

Tensile stress in the concrete is ignored, and therefore the tensile concrete does not contribute to the cross-sectional properties. Material behaviour is linear-elastic. This includes concrete in compression, and both the non-prestressed and prestressed reinforcement.

The two cases of axial force with uniaxial bending and axial force with biaxial bending are dealt with separately in the following sections. 7.2.1 Axial force and uniaxial bending In the short-term analysis of the section at ﬁrst loading (at time τ 0 ), it is assumed that the axial force and bending moment about the x-axis, Ne,0 and Me,0 , respectively, produce tension of sufﬁcient magnitude to cause cracking in the bottom ﬁbres of the cross-section and compression at the top of the section. Consider the cracked partially-prestressed concrete cross-section shown in Fig. 7.4. The section is symmetric about the y-axis and, for convenience, the orthogonal x-axis is selected as the reference axis. Also shown in Fig. 7.4 are the initial stress and strain distributions when the section is subjected to combined bending and axial force (Me.0 and Ne.0 ) sufﬁcient to cause cracking in the bottom ﬁbres. The numbers of layers of non-prestressed and prestressed reinforcement for the cross-section in Fig. 7.4 are ms = 3 and mp = 2, respectively. As for the analysis of uncracked cross-sections in Section 5.3, the properties of each layer of non-prestressed reinforcement are deﬁned by its area, elastic modulus and location with respect to the arbitrarily chosen x-axis, i.e. As(i) , Es(i) and ys(i) (= ds(i) − dref ), respectively. Similarly, Ap(i) , Ep(i) and yp(i) (= dp(i) − dref ) represent the area, elastic modulus and location of the prestressing steel with respect to the x-axis, respectively. The strain at any depth y below the reference x-axis at time τ 0 is given by: ε0 = εr,0 + yκ0

(7.1)

The stresses in the concrete and in the bonded reinforcement are: σc,0 = Ec,0 ε0 = Ec,0 (εr,0 + yκ0 ) for y ≤ yn,0

(7.2a)

σc,0 = 0 for y > yn,0

(7.2b)

ds(1) ds(2)

dref ys(1) ys(2)

As(1) As(2) x

yn,0 dp(1) dp(2)

ds(3)

yp(1) yp(2) ys(3)

Ap(1) Ap(2) As(3)

etop es(1) es(2)

Me,0 Ne,0

eref

stop = Ec,0etop

e

ss(1) ss(2)

s

sp(1) sp(2) ss(3)

es(3)

y (a) Cross-section

(b) Strain diagram

(c) Stress

Figure 7.4 Fully-cracked reinforced concrete cross-section.

Cracked sections 267 σs(i),0 = Es(i) ε0 = Es(i) (εr,0 + ys(i) κ0 ) σp(i),0 = Ep(i) ε0 + εp(i),init = Ep(i) εr,0 + yp(i) κ0 + εp(i),init

(7.3) (7.4)

where yn,0 is the distance from the reference axis to neutral axis, as shown in Fig. 7.4a, and εp(i),init is the strain in the i-th layer of prestressing steel immediately before the transfer of prestress to the concrete as expressed in Eq. 5.5 (reproduced and renumbered here for convenience): Pp(i),init Ap(i) Ep(i)

εp(i),init =

(7.5)

The internal axial force Ni,0 on the cracked cross-section is the sum of the axial forces resisted by the various materials forming the cross-section and is given by: Ni,0 = Nc,0 + Ns,0 + Np,0

(7.6)

where Nc,0 , Ns,0 and Np,0 represent the axial forces resisted by the concrete, the nonprestressed reinforcement and the prestressing steel, respectively, and are calculated using: Nc,0 =

σc,0 dA =

Ac

Ns,0 =

Ec,0 (εr,0 +yκ0 ) dA = Ac Ec,0 εr,0 +Bc Ec,0 κ0

(7.7a)

Ac

ms

ms ms As(i) Es(i) εr,0 +ys(i) κ0 = As(i) Es(i) εr,0 + ys(i) As(i) Es(i) κ0

i=1

i=1

i=1

(7.7b) mp mp mp Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(i) Ep(i) εp(i),init Np,0 = i=1

i=1

(7.7c)

i=1

where Ac and Bc are the area and the ﬁrst moment of area about the x-axis of the compressive concrete above the neutral axis (i.e. the properties of the intact compressive concrete). Adopting the following notation: RA,s =

ms ms ms 2 As(i) Es(i) ;RB,s = ys(i) As(i) Es(i) ;RI,s = ys(i) As(i) Es(i) i=1

RA,p =

i=1

i=1

mp mp mp 2 Ap(i) Ep(i) ;RB,p = yp(i) Ap(i) Ep(i) ;RI,p = yp(i) Ap(i) Ep(i) i=1

i=1

(7.8)

i=1

Eqs 7.7 become Nc,0 =

σc,0 dA =

Ac

Ec,0 (εr,0 + yκ0 )dA

(7.9a)

Ac

Ns,0 = RA.s εr,0 + RB.s κ0

(7.9b)

268 Cracked sections Np,0 = RA,p εr,0 + RB,p κ0 +

mp Ap(i) Ep(i) εp(i),init

(7.9c)

i=1

Remembering that for equilibrium Ne,0 = Ni,0 and that substituting Eqs 7.9 into Eq. 7.6 the expression for Ni,0 can be re-written in terms of the actual geometry and the elastic moduli of the materials forming the cross-section: Ni,0 =

Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 + (RB,s + RB,p )κ0 Ac

+

mp Ap(i) Ep(i) εp(i),init = Ne,0

(7.10)

i=1

Eq. 7.10 can be re-expressed as: mp Ne,0 − Ap(i) Ep(i) εp(i),init = Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 i=1

Ac

+ (RB,s + RB,p )κ0

(7.11)

Similarly, the following expression based on moment equilibrium can be derived as: mp Me,0 − yp(i) Ap(i) Ep(i) εp(i),init = Ec,0 (εr,0 + yκ0 )ydA + (RB,s + RB,p )εr,0 i=1

Ac

+ (RI,s + RI,p )κ0

(7.12)

For a reinforced concrete section comprising rectangular components (e.g. rectangular ﬂanges and webs) loaded in pure bending (i.e. Ne,0 = Ni,0 = 0) and with no prestress, Eq. 7.10 becomes a quadratic equation that can be solved to obtain the location of the neutral axis yn,0 . If the cross-section is prestressed or the axial load Ne,0 is not equal to zero, dividing Eq. 7.12 by Eq. 7.11 gives: Me,0 −

mp 0

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

(Ap(i) Ep(i) εp(i),inst )

i=1 y=y 1 n,0

=

Ec,0 (εr,0 + yκ0 )ydA + (RB,s + RB,p )εr,0 + (RI,s + RI,p )κ0

y=−dref y=y 1 n,0 y=−dref

Ec,0 (εr,0 + yκ0 )dA + (RA,s + RA,p )εr,0 + (RB,s + RB,p )κ0

Cracked sections 269 Dividing top and bottom of the right hand side by κ 0 and recognising that at the axis of zero strain y = yn,0 = −εr,0 /κ0 , the above expression becomes: Me,0 −

mp 0

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

(Ap(i) Ep(i) εp(i),inst )

i=1 y=y 1 n,0

=

Ec,0 (−yn,0 + y)ydA − (RB,s + RB,p )yn,0 + (RI,s + RI,p )

y=−dref y=y 1 n,0

(7.13) Ec,0 (−yn,0 + y)dA − (RA,s + RA,p )yn,0 + (RB,s + RB,p )

y=−dref

and Eq. 7.13 may be solved for yn,0 relatively quickly using a simple trial and error search. When yn,0 is determined, and the depth of the intact compressive concrete above the cracked tensile zone is known, the properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis may be readily calculated. Using the same notation as in the short-term analysis of the uncracked section of Section 5.3 (Eqs 5.8–5.11), the expressions for Ni,0 and Mi,0 (Eqs 7.10 and 7.12) can be rewritten as: Ni,0 = RA,0 εr,0 + RB,0 κ0 +

mp Ap(i) Ep(i) εp(i),init

(7.14a)

i=1 mp

Mi,0 = RB,0 εr,0 + RI,0 κ0 +

yp(i) Ap(i) Ep(i) εp(i),init

(7.14b)

i=1

and RA,0 , RB,0 and RI,0 are the axial rigidity and the stiffness related to the ﬁrst and second moments of area of the cracked section about the reference axis, respectively, calculated at time τ 0 and are given by: RA,0 = Ac Ec,0 +

ms i=1

RB,0 = Bc Ec,0 +

ms

As(i) Es(i) +

mp

Ap(i) Ep(i) = Ac Ec,0 + RA,s + RA,p

(7.15a)

i=1

ys(i) As(i) Es(i) +

i=1

mp

yp(i) Ap(i) Ep(i) = Bc Ec,0 + RB,s + RB,p

i=1

(7.15b) RI,0 = Ic Ec,0 +

ms i=1

mp

2 ys(i) As(i) Es(i) +

2 yp(i) Ap(i) Ep(i) = Ic Ec,0 + RI,s + RI,p (7.15c)

i=1

The system of equilibrium equations governing the problem (Eq. 5.12) is rewritten here as: re,0 = D0 ε0 + fp,init

(7.16)

270 Cracked sections and solving gives the vector of unknown strains: re,0 − fp,init = F0 re,0 − fp,init ε0 = D−1 0

(7.17)

As deﬁned previously:

Ne,0 re,0 = Me,0

RB,0 RI,0

RA,0 D0 = RB,0

εr,0 ε0 = κ0 fp,init =

mp i=1

F0 =

(7.18a) (7.18b)

(7.18c) Ap(i) Ep(i) εp(i),init yp(i) Ap(i) Ep(i) εp(i),init

1 RA,0 RI,0 − R2B,0

RI,0 −RB,0

(7.18d) −RB,0 RA,0

(7.18e)

The stress distribution in the concrete and reinforcement can then be calculated from Eqs 7.2 to 7.4. As an alternative approach, the solution may also be conveniently obtained using the cross-sectional properties of the transformed section. For example, for the cross-section of Fig. 7.4, the transformed cross-section in equivalent areas of concrete for the shortterm analysis is shown in Fig. 7.5. The cross-sectional rigidities of the transformed section deﬁned in Eqs 7.15 can be re-calculated as: RA,0 = A0 Ec,0

(7.19a)

RB,0 = B0 Ec,0

(7.19b)

RI,0 = I0 Ec,0

(7.19c) (ns(1),0 −1)As(1) (ns(2),0 −1)As(2) x yn,0 np(1),0 Ap(1) np(2),0 Ap(2)

if bonded

ns(3),0 As(3) y

Figure 7.5 Transformed cracked section with bonded reinforcement (transformed into equivalent areas of concrete).

Cracked sections 271 where A0 is the area of the transformed cracked concrete section, and B0 and I0 are the ﬁrst and second moments of the transformed area about the reference x-axis at ﬁrst loading. Substituting Eqs 7.19 into Eq. 7.18e, the matrix F0 becomes: F0 =

I0 −B0 Ec,0 (A0 I0 − B20 ) −B0 A0 1

(7.20)

Example 7.1 Assuming that the concrete can carry no tension, the position of the neutral axis and the stress and strain distributions immediately after ﬁrst loading are to be calculated on the reinforced concrete cross-section shown in Fig. 7.6 for each of the following load cases: (1) Ne,0 = 0 and Me,0 = 300 kNm; (2) Ne,0 = −1000 kN and Me,0 = 300 kNm. Both the concrete and the reinforcement are assumed to be linear-elastic with Ec,0 = 25 GPa and Es = 200 GPa. The modular ratio for the reinforcing steel is therefore ns,0 = 8. 1000 100 322

Me,0

x 530

Ne,0

y As = 4000 mm2

70 400

Figure 7.6 Reinforced concrete cross-section for Example 7.1

Load case 1: Ne,0 = 0 and Me,0 = Mi,0 = 300 kNm Initially, it is assumed that the neutral axis is located in the 400 mm wide web of the cross-section. From Eq. 7.8: RA,s = As Es = 4000 × 200,000 = 800 × 106 N RB,s = ys As Es = (630 − 322) × 4000 × 200,000 = 246.4 × 109 Nmm RI,s = ys2 As Es = (630 − 322)2 × 4000 × 200,000 = 75.89 × 1012 Nmm2

272 Cracked sections With Ne,0 = Ni,0 = 0, Eq. 7.10 becomes: Ne,0 =

Ec,0 (εr,0 + yκ0 )dA + RA,s εr,0 + RB,s κ0 = 0 Ac

Dividing by κ 0 and remembering that yr,0 = −εr,0 /κ 0 gives: Ec,0 (−yn,0 + y)dA − RA,s yn,0 + RB,s = 0 Ac

which can be used to obtain a parabolic expressions in yn,0 : y=−222

y=y n,0

25,000(−yn,0 + y) × 1000 dy + y=−322

25,000(−yn,0 + y) × 400 dy

y=−222

− 800 × 106 yn,0 + 246.4 × 109 = 0 −222 yn,0 + 10 × 106 (−yn,0 y + 0.5y2 ) 25 × 106 (−yn,0 y + 0.5y2 ) −322

−222

− 800 × 106 yn,0 + 246.4 × 109 = 0 2 2 + 5yn,0 5550yn,0 + 616,100 − 8050yn,0 − 1,296,000 − 10yn,0

− 2220yn,0 − 246,400 − 800yn,0 + 246,400 = 0 2 + 1104yn,0 + 136,000 = 0 yn,0

Solving this quadratic equation gives yn,0 = −141.3 mm. Therefore the depth of the neutral axis below the top surface is dn = dref + yn,0 = 322 − 141.3 = 180.7 mm and this conﬁrms the earlier assumption that the neutral axis is located in the 400 mm wide web of the section. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 1000 × 100 + 400 × 80.7 = 132,300 mm2 ; Bc = 1000 × 100 × (50 − 322) + 400 × 80.7 × (140.35 − 322) = −33.06 × 106 mm3 ; Ic =

1000 × 1003 400 × 80.73 + 1000 × 100 × (50 − 322)2 + 12 12 + 400 × 80.7 × (140.35 − 322)2 = 8564 × 106 mm4 .

The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s = 132,300 × 25,000 + 800 × 106 = 4107 × 106 N;

Cracked sections 273 RB,0 =Bc Ec,0 +RB,s =−33.06×106 ×25,000+246.4×109 = −580.2×109 Nmm; RI,0 = Ic Ec,0 +RI,s = 8564×106 ×25,000+75.89×1012 = 290.0×1012 Nmm2 .

From Eq. 7.18e: F0 =

1 RA,0 RI,0 −R2B,0

339.4×10−12 679.1×10−15 RI,0 −RB,0 = −RB,0 RA,0 679.1×10−15 4.807 ×10−15

and the strain vector is obtained from Eq. 7.17: 0 339.4×10−12 679.1×10−15 ε0 = F0 re,0 = 300×106 679.1×10−15 4.807 ×10−15 203.7×10−6 = 1.442×10−6 mm−1 From Eq. 7.1, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: ε0(top) = εr,0 − 322 × κ0 = (203.7 − 322 × 1.442) × 10−6 = −260.6 × 10−6 ε0(btm) = εr,0 + 378 × κ0 = (203.7 + 378 × 1.442) × 10−6 = +748.8 × 10−6 The top ﬁbre stress in the concrete and the stress in the reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 25,000×(−260.6×10−6 ) = −6.52 MPa σs,0 =Es (εr,0 +ys κ0 )=200×103 ×(203.7+308×1.442)×10−6 =+129.6 MPa

The results are plotted in Fig. 7.7a. Load case 2: Ne,0 = −1000 kN and Me,0 = 300 kN.m As for load case 1, RA,s = 800×106 N, RB,s = 246.4×109 Nmm, RI,s = 75.89× 1012 Nmm2 , and it is clear that for this load case the depth of the neutral axis is greater than that for load case 1, i.e. yn,0 > −141.3 mm. In this reinforced concrete section, Eq. 7.13 reduces to: y=−y y=−222 1 1 n,0 25,000×1000×(−yn,0 +y)y dy+ 25,000×400×(−yn,0 +y)y dy−246.4×109 yn,0 +75.89×1012 Me,0 y=−322 y=−222 = y=y y=−222 Ne,0 1 1 n,0 25,000×1000×(−yn,0 +y) dy+ 25,000×400×(−yn,0 +y) dy−800×106 yn,0 +246.4×109 y=−322

y=−222

25×106 (−0.5yn,0 y2 +0.3y ˙ 3 )−222 + 10×106 (−0.5yn,0 y2 +0.3y ˙ 3 )yn,0 −246.4×109 yn,0 +75.89×1012 −322 −222 = −222 yn,0 25×106 (−yn,0 y+0.5y2 ) + 10×106 (−yn,0 y+0.5y2 )−222 −800×106 yr,0 +246.4×109 −322 =

3 +680.0×103 y 6 −1.66˙ yn,0 n,0 +299.4×10 2 −5520y 3 −5yn,0 n,0 −680.0×10

= −300 mm

274 Cracked sections Solving this cubic equation (either directly or by trial) gives yn,0 = 85.5 mm. Therefore, the depth of the neutral axis below the top surface is dn = dref +yn,0 = 407.5 mm. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 1000 × 100 + 400 × 307.5 = 223,000 mm2 Bc = 1000 × 100 × (50 − 322) + 400 × 307.5 × (253.8 − 322) = −35.59 × 106 mm3 Ic =

1000 × 1003 400 × 307.53 + 1000 × 100 × (50 − 322)2 + 12 12 + 400 × 307.5 × (253.8 − 322)2 = 9024 × 106 mm4

The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s = 223,000 × 25,000 + 800 × 106 = 6375 × 106 N RB,0 = Bc Ec,0 + RB,s = −35.59 × 106 × 25,000 + 246.4 × 109 = −643.5 × 109 Nmm RI,0 = Ic Ec,0 + RI,s = 9024 × 106 × 25,000 + 75.89 × 1012 = 301.5 × 1012 Nmm2 From Eq. 7.18e: F0 =

1 RA,0 RI,0 −R2B,0

RI,0 −RB,0 199.9×10−12 426.7 ×10−15 = −RB,0 RA,0 426.7 ×10−15 4.228×10−15

and the strain vector is obtained from Eq. 7.17:

199.9 × 10−12 426.7 × 10−15 ε0 = F0 re,0 = 426.7 × 10−15 4.228 × 10−15

−71.9 × 10−6 = 0.842 × 10−6 mm−1

−1000 × 103 300 × 106

From Eq. 7.1, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: ε0(top) = εr,0 −322×κ0 = (−71.9−322×0.842)×10−6 = −343.0×10−6 ε0(btm) = εr,0 +378×κ0 = (−71.9+378×0.842)×10−6 = +246.4×10−6

Cracked sections 275 1000 −6.52

−260.6 100 180.7 Neutral axis

+648.0

129.6

+748.8 Strain × 10−6 Stress (MPa)

Cross-section

(a) Load case 1: Ne,0 = 0 and Me,0 = 300 kN.m.

1000 −343.0

−8.57

100 407.5 Neutral axis +187.3

Cross-section

+246.4 Strain × 10−6

37.5

Stress (MPa)

(a) Load case 2: Ne,0 = −1000 kN and Me,0 = 300 kN.m.

Figure 7.7 Initial stress and strain distributions in Example 7.1.

The top ﬁbre stress in the concrete and the stress in the reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 25,000 × (−343.0 × 10−6 ) = −8.57 MPa σs,0 = Es (εr,0 + ys κ0 ) = 200 × 103 × (−71.9 + 308 × 0.842) × 10−6 = +37.5 MPa The results are plotted in Fig. 7.7b.

Example 7.2 The depth of the concrete compression zone dn and the short-term stress and strain distributions are to be calculated on the partially-prestressed concrete beam cross-section shown in Fig. 7.8a, when Me,0 = 400 kNm (and Ne,0 = 0). The section contains two layers of non-prestressed reinforcement as shown (each with Es = 2 × 105 MPa) and one layer of bonded prestressing steel (Ep = 2 × 105 MPa). The prestressing force before transfer is Pp,init = 900 kN = 3.5 MPa (i.e. σp,init = 1200 MPa). The tensile strength of the concrete is fct.f and the elastic modulus is Ec,0 = 30,000 MPa.

276 Cracked sections From Eq. 7.8: RA,s = (As(1) +As(2) )Es = (500+1000)×200,000 = 300×106 N RB,s = (ys(1) As(1) +ys(2) As(2) )Es = (−250×500+400×1000)×200,000 = 55.0×109 Nmm 2 2 RI,s = (ys(1) As(1) +ys(2) As(2) )Es = ((−250)2 ×500+4002 ×1000)×200,000

= 38.25×1012 Nmm2 RA,p = Ap Ep = 750×200,000 = 150×106 N RB,p = yp Ap Ep = 275×750×200,000 = 41.25×109 Nmm RI,p = yp2 Ap Ep = (275)2 ×750×200,000 = 11.34×1012 Nmm2 The strain in the prestressing steel caused by Pp,init before transfer is given by Eq. 7.5: εp(i),init =

900 × 103 = 6000 × 10−6 750 × 2 × 105

and the vector of actions due to initial prestress is given by Eq. 7.18d:

750 × 200,000 × 0.006 900 × 103 N fp,init = = 275 × 750 × 200,000 × 0.006 247.5 × 106 Nmm If it is initially assumed that the section is uncracked, an analysis using the procedure outlined in Section 5.3 indicates that the tensile strength of the concrete has been exceeded in the bottom ﬁbres of the cross-section. With the reference axis selected at dref = 300 mm below the top of the section, the depth of the neutral axis below the reference axis yn,0 is determined from Eq. 7.13. The left hand side of Eq. 7.13 is ﬁrst calculated: mp 0

Me,0 −

(yp(i) Ap(i) Ep(i) εp(i),inst )

i=1 mp 0

Ne,0 −

= (Ap(i) Ep(i) εp(i),inst )

400×106 −247.5×106 = −169.4˙ mm 0−900×103

i=1

and therefore: y=y 1 n,0

−169.4 =

30,000 × 200 × (−yn,0 + y)y dy − (55.0 + 41.25) × 109 yn,0 + (38.25 + 11.34) × 1012

y=−300 y=y 1 n,0

30,000 × 200 × (−yn,0 + y)dy − (300 + 150) × 106 yn,0 + (55.0 + 41.25) × 109

y=−300

−169.4 =

6.0 × 106 (−0.5yn,0 y2 + 0.3y ˙ 3 )yn,0 − 96.25 × 109 yn,0 + 49.59 × 1012 y−300 6.0 × 106 (−yn,0 y + 0.5y2 ) n,0 − 450 × 106 yn,0 + 96.25 × 109 −300

−169.4 =

3 + 173,750y 6 −yn,0 n,0 + 103.6 × 10 2 −3yn,0 − 2250yn,0 − 173,750

Cracked sections 277 Solving gives yn,0 = 208.1 mm. Therefore the depth of the neutral axis below the top surface is dn = dref + yn,0 = 508.1 mm. The properties of the compressive concrete (Ac , Bc and Ic ) with respect to the reference axis are: Ac = 508.1×200−500 = 101,100 mm2 Bc = 508.1×200×(254.05−300)−500×(50−300) = −4.55×106 mm3 Ic =

200×508.13 +200×508.1×(254.05−300)2 −500×(50−300)2 12

= 2370×109 mm4 The cross-sectional rigidities RA,0 , RB,0 and RI,0 are obtained from Eqs 7.15: RA,0 = Ac Ec,0 + RA,s + RA,p = 101,120 × 30,000 + 300 × 106 + 150 × 106 = 3484 × 106 N RB,0 = Bc Ec,0 + RB,s + RB,p = −4.55 × 106 × 30,000 + 55.0 × 109 + 41.25 × 109 = −40.24 × 109 Nmm RI,0 = Ic Ec,0 + RI,s + RI,p = 2370 × 106 × 30,000 + 38.25 × 1012 + 11.34 × 1012 = 120.7 × 1012 Nmm2 From Eq. 7.18e: F0 =

1

RI,0 −RB,0

RA,0 RI,0 −R2B,0 −RB,0 RA,0

=

288.1×10−12 96.06×10−15

96.06×10−15 8.317 ×10−15

and the strain vector is obtained from Eq. 7.17:

288.1 × 10−12 96.06 × 10−15 × ε0 = F0 re,0 − fp,init = 96.06 × 10−15 8.317 × 10−15

−244.6 × 10−6 0 − 900 × 103 = × 400 × 106 − 247.5 × 106 1.182 × 10−6 mm−1 From Eq. 7.1, the top (y = −300 mm) and bottom (y = +450 mm) ﬁbre strains are: ε0(top) = εr,0 − 300 × κ0 = (−244.6 − 300 × 1.182) × 10−6 = −599.1 × 10−6 ε0(btm) = εr,0 + 450 × κ0 = (−244.6 + 450 × 1.182) × 10−6 = +287.3 × 10−6

278 Cracked sections The distribution of strains is shown in Fig. 7.8b. 50

200

As(1) = 500 mm2

−599

−18.0 −108.1

dref = 300

Me,0 = 400 kN.m

575 700

508.1

x Neutral axis

Ap = 750 mm2

1216 Pp,init = 900 kN 45.6

As(2) = 1000 mm2 287

50 (a) Section

(b) Strain (× 10−6)

(c) Stress (MPa)

Figure 7.8 Cross-sectional details and stress and strain distributions for Example 7.2 (all dimensions in mm).

The top ﬁbre stress in the concrete and the stress in the non-prestressed reinforcement are (Eqs 7.2a and 7.3): σc,0(top) = Ec,0 ε0(top) = 30,000 × (−599.1 × 10−6 ) = −18.0 MPa σs(1),0 = Es (εr,0 + ys(1) κ0 ) = 200 × 103 × (−244.6 − 250 × 1.182) × 10−6 = −108.1 MPa σs(2),0 = Es (εr,0 + ys(2) κ0 ) = 200 × 103 × (−244.6 + 400 × 1.182) × 10−6 = +45.6 MPa and the stress in the prestressing steel is given by: σp,0 = Ep εr,0 + yp κ0 + εp,init = 200 × 103 × (−244.6 + 275 × 1.182 + 6000) × 10−6 = 1216 MPa The stresses are plotted in Fig. 7.8c. 7.2.2 Axial force and biaxial bending The short-term analysis of an uncracked cross-section subjected to axial force and biaxial bending was presented in Section 6.2. The procedure is readily extended to cracked sections where the extent of cracking is evaluated based on a trial and error procedure depicted in Fig. 7.9 and described below. In the ﬁrst iteration, all concrete is initially assumed to be uncracked (Fig. 7.9a) and the analysis is identical to that described in Section 6.2. If the maximum tensile

Cracked sections 279

x

x

y

x

y

Neutral axis

Neutral axis

e

e (a) Iteration 1

(b) Iteration 2

y

Neutral axis

e (c) Iteration 3

Figure 7.9 Iterative procedure for cracked sections under axial force and biaxial bending.

stress in the concrete exceeds the tensile strength of the concrete, cracking is deemed to have occurred. In this case, the area of concrete in tension identiﬁed after the ﬁrst iteration is assumed to be cracked and to no longer contribute to the stiffness of the cross-section. This occurs, for example, in the bottom left hand corner of the cross-section shown in Fig. 7.9a, where the triangular part of the concrete section on the tensile side of the neutral axis is identiﬁed to have cracked. For the second iteration, the solution procedure remains unchanged except that the contribution of the concrete to the cross-sectional rigidities changes, with the cracked area of concrete identiﬁed in the ﬁrst iteration (shown as the unshaded region in Fig. 7.9b) now not included in the calculation of the concrete section properties (Ac , Bxc , Byc , Ixc , Iyc , Ixyc ). After the second iteration, the revised neutral axis location is determined and a new area of cracked concrete is calculated. This procedure is continued in successive iterations (Fig. 7.9c) until the differences in the calculated cross-sectional rigidities between successive iterations are negligible. From a numerical viewpoint, convergence is usually assumed to have occurred when the variations of the values of the variables deﬁning the strain diagram (i.e. ε r , κ x and κ y ) in consecutive iterations are negligible.

7.3 Time-dependent analysis (AEMM) In the analyses presented here, the fully-cracked cross-sectional area (i.e. the size of the uncracked concrete compressive zone) is assumed to remain constant with time. This assumption is not correct since creep causes a gradual change of the position of the neutral axis under sustained loads. However, as discussed in Section 7.1, the assumption greatly simpliﬁes the analysis and will usually result in relatively little error in the calculated deformations. 7.3.1 Axial force and uniaxial bending With the depth of the concrete compression zone dn assumed to remain constant with time, the time analysis of a fully-cracked cross-section using the AEMM is essentially the same as that outlined in Section 5.4.

280 Cracked sections

ds(2)

ds(1)

etop,0

etop,k As(1) As(2)

dn

x

dref

Me,k

k0 Ne,k kk

dp(1)

Ap(1) Ap(2) As(3)

dp(2) ds(3) (a) Cross-section

(b) Strain

Figure 7.10 Fully-cracked cross-section – time analysis (AEMM).

The fully-cracked cross-section shown in Fig. 7.10a is subjected to a sustained external bending moment Me,0 and axial force Ne,0 . Both the short-term and time-dependent strain distributions are shown in Fig. 7.10b. For the time analysis, the steel reinforcement and prestressing tendons (if any) are assumed to be linear-elastic (as for the short-term analysis) and the constitutive relationship for the concrete at τ k is that given by Eq. 4.45. Therefore: σc,k = Ee,k εk − εsh,k + Fe,0 σc,0 for y ≤ yn,0 and σc,k = 0 for y > yn,0 (7.21a) σs(i),k = Es(i) εk

(7.21b)

σp(i),k = Ep(i) εk + εp(i),init − εp.rel(i),k

(7.21c)

where Ee,k , Fe,0 and ε p.rel(i),k are as deﬁned previously (and given in Eqs 4.35, 4.46 and 5.23a). At time τ k , the internal axial force Ni,k and moment Mi,k on the cross-section are given in Eqs 5.29 and 5.31 and the axial rigidity and the stiffness related to the ﬁrst and second moments of area (RA,k , RB,k , and RI,k , respectively) are given by Eqs 5.30 and 5.32. The equilibrium equations are expressed in Eq. 5.34 and solving using Eq. 5.39 gives the strain vector at time τ k . The stresses in the concrete, steel reinforcement and tendons at time τ k are then calculated from Eqs 5.41a, b and c, respectively.

Example 7.3 The change of stress and strain with time on the cracked cross-section of Example 7.1 (Fig. 7.6) is to be calculated using AEMM. Each of the loading cases considered in Example 7.1 is to be examined here. The relevant material properties for the time period in question are: Ec,0 = 25 GPa; Es = 200 GPa; ϕ(τk , τ0 ) = 3.0; χ (τk , τ0 ) = 0.65; εsh (τk ) = −500 × 10−6 and the steel reinforcement is assumed to be linear elastic. To illustrate the effects of creep, the case when εsh (τk ) = 0 is also to be considered for load case 1.

Cracked sections 281 Load case 1a: Ne,k = 0; Me,k = Mi,k = 300 kNm and εsh (τk ) = −500 × 10−6 From load case 1 in Example 7.1, dn = 180.7 mm; εr,0 = 203.7 × 10−6 ; κ0 = 1.442 × 10−6 mm−1 ; and the shape of the cracked cross-section and the initial stress and strain distributions are illustrated in Fig. 7.7a. From Eqs 4.35 and 4.46: Ee,k =

Ec,0 25,000 = = 8475 MPa 1 + χ(τk , τ0 )ϕ(τk , τ0 ) 1 + 0.65 × 3.0

ϕ (τk , τ0 ) [χ (τk , τ0 ) − 1] 3.0 × (0.65 − 1.0) = −0.356 Fe,0 = = 1 + χ (τk , τ0 ) ϕ (τk , τ0 ) 1.0 + 0.65 × 3.0 and as calculated in Example 7.1, the properties of the concrete part of the cross-section with respect to the reference axis are Ac = 132,300 mm2 , Bc = −33.06 × 106 mm3 and Ic = 8564 × 106 mm4 and the rigidities of the steel reinforcement are RA,s = 800 × 106 N, RB,s = 246.4 × 109 Nmm and RI,s = 75.89 × 1012 Nmm2 . The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −518.3 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +140.4 × 106 Nmm The cross-sectional rigidities RA,k , RB,k and RI,k are obtained from Eqs 5.30 and 5.32: RA,k = Ac Ee,k + RA,s = 132,300 × 8475 + 800 × 106 = 1921 × 106 N Ee,k + RB,s = −33.06 × 106 × 8475 + 246.4 × 109 RB,k = Bc = −33.78 × 109 Nmm Ee,k + RI,s = 8564 × 106 × 8475 + 75.89 × 1012 RI,k = Ic = 148.5 × 1012 Nmm2 From Eq. 5.40: Fk =

1 RA,k RI,k −R2B,k

RI,k −RB,k 522.7 ×10−12 118.9×10−15 = −RB,k RA,k 118.9×10−15 6.761×10−15

and from Eqs 5.36 and 5.37: fcr,k = Fe,0

Nc,0 Mc,0

−518.1 × 103 = −0.356 × +145.4 × 106

+184.5 × 103 = −49.96 × 106

282 Cracked sections

Ac 132,300 fsh,k = Ee,k εsh,k = × 8475 × (−500 × 10−6 ) Bc −33.06 × 106

−560.6 × 103 = +140.1 × 106 For this reinforced concrete cross-section, the strain vector is obtained from Eq. 5.39: εk = Fk re,k − fcr,k + fsh,k 522.7 × 10−12 118.9 × 10−15 (0 − 184.5 − 560.6) × 103 = 118.9 × 10−15 6.761 × 10−15 (300 + 49.96 + 140.1) × 106

−331.0 × 10−6 = 3.225 × 10−6 mm−1

From Eq. 5.20, the top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are: εk(top) = εr,k −322×κk = (−331.0−322×3.225)×10−6 = −1370×10−6 εk(btm) = εr,k +378×κk = (−331.0+378×3.225)×10−6 = +888×10−6 The concrete stresses at time τk at the top ﬁbre (y = −322 mm) and at the bottom of the compressive concrete, at yn,0 = −141.3 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−1370 + 500) × 10−6 − 0.356 × −6.52 = −5.05 MPa At yn,0 = −141.3 mm: σc,k = 8475 × (−331.0 − 141.3 × 3.225 + 500) × 10−6 − 0.356 × 0 = −2.43 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−331.0 + 308 × 3.225) × 10−6 = +132.5 MPa The results are plotted in Fig. 7.11a. Load case 1b: Ne,k = 0; Me,k = 300 kNm and εsh (τk ) = 0 The only difference from load case 1a, is that the shrinkage vector is now nil, that is, fsh,k = 0, and from Eq. 5.39, the strain vector is now: εk = Fk re,k − fcr,k + fsh,k

Cracked sections 283

522.7 × 10−12 118.9 × 10−15 (0 − 184.5 + 0) × 103 εk = 118.9 × 10−15 6.761 × 10−15 (300 + 49.96 + 0) × 106

−54.8 × 10−6 = 2.344 × 10−6 mm−1

The top and bottom ﬁbre strains are: εk(top) = εr,k − 322 × κk = (−58.8 − 322 × 2.344) × 10−6 = −810 × 10−6 εk(btm) = εr,k + 378 × κk = (−58.8 + 378 × 2.344) × 10−6 = +831 × 10−6 The concrete stresses at time τ k at the top ﬁbre and at the bottom of the compressive concrete, at yn,0 = −141.3 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−810) × 10−6 − 0.356 × −6.52 = −4.54 MPa At yn,0 = −141.3 mm: σc,k = 8475 × (−58.8 − 141.3 × 2.344) × 10−6 − 0.356 × 0 = −3.27 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−58.8 + 308 × 2.344) × 10−6 = +133.5 MPa The results are plotted in Fig. 7.11b. The effects of shrinkage acting alone are obtained by subtracting the strains and stresses calculated for load case 1b from those for load case 1a and the results are plotted in Fig. 7.11c. Load case 2: Ne,0 = −1000 kN, Me,0 = 300 kNm and εsh (τk ) = −500 × 10−6 From load case 2 in Example 7.1, dn = 407.5 mm; εr,0 = −71.9 × 10−6 ; κ0 = 0.842 × 10−6 mm−1 and the initial stress and strain distributions are illustrated in Fig. 7.7b. As for load case 1: Ee,k = 8475 MPa and Fe,0 = −0.356. As calculated in Example 7.1, the properties of the concrete part of the cross-section with respect to the reference axis are Ac = 223,000 mm2 , Bc = −35.59 × 106 mm3 and Ic = 9024 × 106 mm4 and the rigidities of the steel reinforcement are RA,s = 800 × 106 N, RB,s = 246.4 × 109 Nmm and RI,s = 75.89 × 1012 Nmm2 . The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −1150 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +253.9 × 106 Nmm

284 Cracked sections The cross-sectional rigidities RA,k , RB,k and RI,k are obtained from Eqs 5.30 and 5.32: RA,k = Ac Ee,k + RA,s = 223,000 × 8475 + 800 × 106 = 2690 × 106 N Ee,k + RB,s = −35.59 × 106 × 8475 + 246.4 × 109 RB,k = Bc = −55.23 × 109 Nmm Ee,k + RI,s = 9024 × 106 × 8475 + 75.89 × 1012 RI,k = Ic = 152.4 × 1012 Nmm2 From Eq. 5.40: Fk =

1 RA,k RI,k − R2B,k

RI,k −RB,k 374.5 × 10−12 135.7 × 10−15 = −RB,k RA,k 135.7 × 10−15 6.611 × 10−15

and from Eqs 5.36 and 5.37:

Nc,0 −1150 × 103 +409.3 × 103 Fe,0 = −0.356 × = fcr,k = Mc,0 +253.9 × 106 −90.36 × 106

223,000 Ac fsh,k = Ee,k εsh,k = × 8475 × −500 × 10−6 Bc −35.59 × 106

−945.0 × 103 = +150.8 × 106 The strain vector is obtained from Eq. 5.39: εk = Fk re,k − fcr,k + fsh,k

(−1000 − 409.3 − 945.0) × 103 374.5 × 10−12 135.7 × 10−15 = 135.7 × 10−15 6.611 × 10−15 (300 + 90.36 + 150.8) × 106

−808.3 × 10−6 = 3.258 × 10−6 mm−1 The top (y = −322 mm) and bottom (y = +378 mm) ﬁbre strains are therefore: εk(top) = εr,k −322×κk = (−808.3−322×3.258)×10−6 = −1857 ×10−6 εk(btm) = εr,k +378×κk = (−808.3+378×3.258)×10−6 = +423×10−6 The concrete stresses at time τk at the top ﬁbre (y=−322 mm) and at the bottom of the compressive concrete, at yn,0 = +85.5 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 8475 × (−1857 + 500) × 10−6 − 0.356 × −8.57 = −8.45 MPa

Cracked sections 285 At yn,0 = +80.5 mm: σc,k = 8475 × (−808.3 + 85.5 × 3.258 + 500) × 10−6 − 0.356 × 0 = −0.39 MPa The stress in the reinforcement is: σs,k = Es (εr,k + ys κk ) = 200 × 103 × (−808.3 + 308 × 3.258) × 10−6 = +39.0 MPa The results are plotted in Fig. 7.11d. −1370

−6.52 −5.05

−261

t0

−810

−261

−6.52 −4.54 t0

−2.43

−3.27

tk

tk

+129.6 at t0

+129.6 at t0 +132.5 at tk

+749 +888 Strain × 10−6

Strain × 10−6

Stress (MPa)

−8.57 −8.45

−343

−1857

−0.51

Stress (MPa)

(b) Load case 1b (creep only)

(a) Load case 1a (creep + shrinkage) −560

+133.5 at tk

+749 +831

t0

+0.84 tk

tk

0.39 +37.5 at t0 +57 Strain × 10−6

−1.0 at tk Stress (MPa)

(c) Load case 1c (shrinkage only)

+246 +423 Strain × 10−6

+39.0 at tk Stress (MPa)

(d) Load case 2 (creep + shrinkage)

Figure 7.11 Stress and strain distributions for Example 7.3.

Example 7.4 The change of stress and strain with time on the cracked partially-prestressed cross-section of Example 7.2 (Fig. 7.8) is to be calculated using AEMM. The actions on the section are assumed to be constant throughout the time period under consideration (i.e. τ0 to τk ) and equal to Ne,k = 0; Me,k = 400 kN.m. The relevant material properties: Ec,0 = 30 GPa; Es = Ep = 200 GPa; ϕ(τk , τ0 ) = 2.5; χ(τk , τ0 ) = 0.65; εsh (τk ) = −400 × 10−6 ; ϕ(τk , σp(i),init ) = 0.02 and the steel reinforcement is assumed to be linear elastic. From Example 7.2: dn = 508.1 mm, εr,0 = −244.6 × 10−6 , κ0 = 1.182 × 10−6 mm−1 , Ac = 101,100 mm2 , Bc = −4.55 × 106 mm3 , Ic = 2370 × 106 mm4

286 Cracked sections and the rigidities of the steel reinforcement and tendons are RA,s = 300 × 106 N, RB,s = 55.0 × 109 Nmm, RI,s = 38.25 × 1012 Nmm2 , RA,p = 150 × 106 N, RB,p = 41.25 × 109 Nmm and RI,p = 11.34 × 1012 Nmm2 . From Eqs 4.35 and 4.46: Ee,k =

30,000 = 11,430 MPa 1 + 0.65 × 2.5

and 2.5 × (0.65 − 1.0) Fe,0 = = −0.333 1.0 + 0.65 × 2.5 The axial force and moment resisted by the concrete part of the cross-section at time τ0 are: Nc,0 = Ac Ec,0 εr,0 + Bc Ec,0 κ0 = −903.2 × 103 N Mc,0 = Bc Ec,0 εr,0 + Ic Ec,0 κ0 = +117.4 × 106 N.mm The cross-sectional rigidities RA,k , RB,k and RI,k are: RA,k = Ac Ee,k + RA,s + RA,p = 101,100 × 11,430 + 300 × 106 + 150 × 106 = 1606 × 106 N Ee,k + RB,s + RB,p = −4.55 × 106 × 11,430 + 55.0 × 109 RB,k = Bc + 41.25 × 109 = 44.24 × 109 Nmm Ee,k + RI,s + RI,p = 2370 × 106 × 11,430 + 38.25 × 1012 RI,k = Ic + 11.34 × 1012 = 76.68 × 1012 Nmm2 and from Eq. 5.40: Fk =

1 RA,k RI,k −R2B,k

RI,k −RB,k 632.7 ×10−12 −365.1×10−15 = −RB,k RA,k −365.1×10−15 13.25×10−15

From Eqs 5.36 to 5.38:

Nc,0 −903.2 × 103 +301.1 × 103 ˙ fcr,k = Fe,0 = −0.333 × = Mc,0 +117.4 × 106 −39.13 × 106

Ac 101,100 fsh,k = Ee,k εsh,k = × 11,430 × −400 × 10−6 Bc −4.55 × 106 −462.2 × 103 = +20.80 × 106

Cracked sections 287 mp

Ap(i) Ep(i) 900 × 103 fp,init = ε = (from Example 7.2) yp(i) Ap(i) Ep(i) p(i),init 247.5 × 106 i=1

18 × 103 fp.rel,k = fp.init ϕp (τk , σp(i),init ) = 4.95 × 106 The strain vector is obtained from Eq. 5.39: εk = Fk re,k −fcr,k +fsh,k −fp,init +fp.rel,k

632.7×10−12 −365.1×10−15 εk = × −365.1×10−15 13.25×10−15

−1120×10−6 (0−301.1−462.2−900+18)×103 = (400+39.13+20.80−247.5+4.95)×106 3.481×10−6 mm−1 The top (y = −300 mm) and bottom (y = +450 mm) ﬁbre strains are: εk(top) = εr,k − 300 × κk = (−1120 − 300 × 3.481) × 10−6 = −2165 × 10−6 εk(btm) = εr,k + 450 × κk = (−1120 + 450 × 3.481) × 10−6 = +446.2 × 10−6 The concrete stresses at time τk at the top ﬁbre (y = −300 mm) and at the bottom of the compressive concrete, at yn,0 = 208.1 mm, are obtained from Eq. 7.21a: At top of section: σc,k = 11,430 × (−2165 + 400) × 10−6 − 0.333 × −18.0 = −14.2 MPa At yn,0 = +208.1 mm: σc,k = 11,430 × (−1120 + 208.1 × 3.481 + 400) × 10−6 − 0.333˙ × 0 = +0.05 MPa The stress in the non-prestressed reinforcement are (Eq. 7.21b): σs(1),0 = Es (εr,0 + ys(1) κ0 ) = 200 × 103 × (−1120 − 250 × 3.481) × 10−6 = −398 MPa σs(2),0 = Es (εr,0 + ys(2) κ0 ) = 200 × 103 × (−1120 + 400 × 3.481) × 10−6 = +54.4 MPa and the stress in the prestressing steel is given by (Eq. 7.21c): σp,0 = Ep εr,0 + yp κ0 + εp.init + εp.rel,k = 200 × 103 × (−1120 + 275 × 3.481 + 6000 − 120) × 10−6 = +1143 MPa

288 Cracked sections The results are plotted in Fig. 7.12. 200 −2165

−599 tk

dref = 300

−18.0 −14.2 t0

508.1 750

−108 at t0 (−398 at tk)

t0

tk x

Me,k = 400 kN.m 0 +0.05

Pp,init = 900 kN

+1216 at t0 (+1143 at tk) +45.6 at t0 (+54.4 at tk)

287 446

Figure 7.12 Initial and time-dependent strain and stress distributions for Example 7.4 (all dimensions in mm).

7.3.2 Axial force and biaxial bending The procedure required for the time analysis of a cracked section in biaxial bending using the AEMM is identical to that for an uncracked section as presented in Section 6.3 and, for this reason, is not repeated here. The only difference is that the concrete cross-sectional properties are determined based on the shape of the cracked section identiﬁed in the instantaneous analysis. As already discussed, when modelling the timedependent behaviour of a cracked section using the AEMM, it is convenient to assume that the area of uncracked concrete does not vary with time. For most purposes, this assumption is quite reasonable and does not result in signiﬁcant error. More reﬁned computer-based methods of analysis can be used to trace the time-varying position of the neutral axis and the gradual change in shape of the cracked area of the cross-section. Such methods are discussed in the following section.

7.4 Short- and long-term analysis using the step-by-step method In some situations, time analysis of a cracked section using the AEMM may not be appropriate. For example, where the section is subjected to a complex load history, it may be necessary to use a more reﬁned analysis. A reﬁned method for the time analysis of a cracked section is described below for the cases of axial force combined with uniaxial and biaxial bending. To avoid unnecessary repetitions reference is made to the derivations presented in previous chapters. 7.4.1 Axial force and uniaxial bending 7.4.1.1 Instantaneous analysis To trace the change of position of the neutral axis and the change in shape of the cracked portion of the cross-section with time, it is convenient to subdivide the concrete

Cracked sections 289 b ds1

As1

dref x

dp1 ds2

y(i) Ap1 Ac(i)

tc(i) As2 y

Figure 7.13 Layered cross-section subjected to axial force and uniaxial bending.

into layers as shown in Fig. 7.13. With this approach, the internal actions, i.e. axial force and moment, are calculated by summing the contributions of each of the layers. Assuming that the cross-section is subdivided into mc concrete layers, and initially assuming that all concrete layers are uncracked, the contribution of the concrete component to the internal axial force Ni,0 previously introduced in Eq. 7.6 can be obtained as follows: mc

Nc,0 =

i=1 mc

=

Ac(i) σc,0 =

mc

Ac(i) Ec(i),0 (εr,0 + y(i) κ0 )

i=1 mc Ac(i) Ec(i),0 εr,0 + Bc(i) Ec(i),0 κ0

i=1

(7.22)

i=1

where Ac(i) and Bc(i) are the area and the ﬁrst moment of area of the i-th concrete layer about the x-axis; y(i) is the distance between the centroid of the i-th concrete layer and the reference axis (Fig. 7.13). This approach assumes that a constant stress is resisted by each layer calculated based on the strain measured at its centroid. Although not used here, a linearly varying stress across the thickness of each layer (t(i) ) can easily be implemented. Similarly, the contribution of the concrete to the internal moment Mi,0 is given by: Mc,0 = =

mc i=1 mc i=1

y(i) Ac(i) σc,0 =

mc

2 Ac(i) Ec(i),0 (y(i) εr,0 + y(i) κ0 )

i=1 mc Bc(i) Ec(i),0 εr,0 + Ic(i) Ec(i),0 κ0

(7.23)

i=1

where Ic(i) is the second moment of area of the i-th concrete layer about the x-axis. The concrete rigidities for the cross-section are: RA,c =

mc mc mc 2 Ac(i) Ec(i),0 ;RB,c = yc(i) Ac(i) Ec(i),0 ;RI,c = yc(i) Ac(i) Ec(i),0 i=1

i=1

i=1

(7.24a,b,c)

290 Cracked sections and the axial force and moment carried by the concrete are re-written as: Nc,0 = RA.c εr,0 + RB.c κ0

(7.25a)

Mc,0 = RB.c εr,0 + RI.c κ0

(7.25b)

In the determination of the properties of each concrete layer (Ac(i) , Bc(i) and Ic(i) ), the concrete displaced by the presence of any reinforcement or tendons in a layer is often ignored, but it is usually straightforward to include the actual concrete area rather than the gross area of the concrete layer. The number of layers (mc ) to be speciﬁed at the beginning of the analysis should be sufﬁcient to produce accurate results. A simple approach to determine mc is to compare the values for the cross-sectional ﬂexural rigidity RI,0 calculated considering the uncracked cross-section with and without layers. The number of layers is acceptable when the difference between these two values is less than 1 per cent. The governing equilibrium equations for a typical cross-section are therefore: Ni,0 = (RA,c + RA,s + RA,p )εr,0 + (RB,c + RB,s + RB,p )κ0 +

mp Ap(i) Ep(i) εp(i),init = Ne,0

(7.26a)

i=1

Mi,0 = (RB,c + RB,s + RB,p )εr,0 + (RI,c + RI,s + RI,p )κ0 mp yp(i) Ap(i) Ep(i) εp(i),init = Me,0 +

(7.26b)

i=1

where the concrete rigidities are given by Eq. 7.24 and the rigidities of the reinforcement and the tendons are deﬁned in Eqs 7.8. This system of two equations can be used to solve for the two unknowns εr,0 and κ0 . To determine the extent of cracking, the solution process is iterative. For the ﬁrst iteration all concrete layers are assumed to be uncracked, that is, each concrete layer contributes to the cross-sectional stiffness. The cross-section is analysed and the concrete stress at the centroid of each layer is determined. For the second iteration, concrete layers subjected to tension in the ﬁrst iteration in excess of the tensile strength of concrete are assumed to have cracked and are subsequently neglected, i.e. the value Ec(i),0 in a cracked layer is set to zero. At the end of each subsequent iteration the stresses are checked in the uncracked layers to identify whether any additional layers have cracked. The short-term analysis is terminated when no additional cracking is detected. More reﬁned material models could be implemented, including the effects of tension-stiffening, tension-softening or other material nonlinearities, and more efﬁcient solving strategies could be used. 7.4.1.2 Time analysis The step-by-step method (SSM) of analysis is adopted. The time discretisation associated with the method was discussed in Section 4.3.1 and the analysis of uncracked cross-sections was presented in Section 5.5, with the constitutive relationships for the concrete, reinforcement and tendons given in Eqs 4.25 and 5.44.

Cracked sections 291 The steps required for the long-term analysis of a cracked section are similar to those required for an uncracked section. The only difference in this case is that the concrete in a cracked layer is assumed to carry no tension. For the layered section of Fig. 7.13, the axial force and moment carried by the concrete to be included in the expression for the internal actions (Eqs 5.50 and 5.51) and the equilibrium equations (Eq. 5.54) can be calculated from:

Nc,j =

mc i=1

=

mc

Ac(i) σc(i),j = ⎛

mc

⎛

⎞ j−1 ⎝Ac(i) Ec(i),j ε(i),j − εsh,j + Fe,j,n σc(i),n Ac(i) ⎠

i=1

n=0

⎝Ac(i) Ec(i),j εr,j + Bc(i) Ec(i),j κj − Ac(i) Ec(i),j εsh,j +

i=1

Mc,j =

mc i=1

=

mc

j−1

⎞ Fe,j,n σc(i),n Ac(i) ⎠

n=0

y(i) Ac(i) σc(i),j = ⎛

mc

⎛

j−1

(7.27a) ⎞

⎝y(i) Ac(i) Ec(i),j ε(i)j − εsh,j + Fe,j,n σc(i),n y(i) Ac(i) ⎠

i=1

⎝Bc(i) Ec(i),j εr,j + Ic(i) Ec(i),j κj − Bc(i) Ec(i),j εsh,j +

i=1

i=0 j−1

⎞

Fe,j,n σc(i),n Bc(i) ⎠

n=0

(7.27b) where the stress history of each layer is recorded separately and the contribution of all cracked layers is zero. As for the instantaneous analysis, an iterative procedure is adopted at each time step. During any iteration, if cracking is detected in a previously uncracked concrete layer (i.e. if the stress at the centroid of the layer exceeds the tensile strength of concrete), the contribution to the cross-sectional rigidities of the concrete in that layer is set to zero and the previous stress history for that layer is subsequently ignored. If the stress in a previously cracked layer becomes compressive, the crack is deemed to have closed and the concrete in the layer begins to contribute to the cross-sectional stiffness and, for the purposes of subsequent creep calculations, the stress history for the layer is stored from this point in time. The iterative procedure continues until the changes in the calculated strain diagram (i.e. the changes in εr,j and κj ) from one iteration to the next are sufﬁciently small. 7.4.2 Axial force and biaxial bending The geometric discretisation required for the analysis of a cross-section subjected to combined axial force and biaxial bending is shown in Fig. 7.14. The cross-section is subdivided both horizontally and vertically into smaller rectangular areas (similar to the layers introduced in the previous section for the case of uniaxial bending). In each rectangular concrete area, the stress is assumed to be constant and is calculated from the strain measured at its centroid. A linearly varying stress distribution could also be considered based on strain values calculated at each corner of the subdivision.

292 Cracked sections

x

y(i)

Ac(i) y

x(i)

Figure 7.14 Geometric discretisation of cross-section - axial force and biaxial bending.

As suggested previously, the ﬁneness of the subdivision to be used for the analysis can be determined by comparing the values of the uncracked ﬂexural rigidities RIx,k , RIy,k and RIxy,k calculated with and without the subdivisions. When the differences are less than 1 per cent, the degree of discretisation is acceptable. The solution process for cracked sections in biaxial bending is identical to that described in Section 7.4.1. In the ﬁrst iteration of the instantaneous analysis, all concrete is assumed to be uncracked. The cracked areas of concrete are identiﬁed and ignored in the next and subsequent iterations. This iterative procedure is applied at each time step, where the effects of creep from the previously stored stress history in each subdivision and the effects of shrinkage are determined. Further changes in the extent of cracking are identiﬁed at the end of each iteration, as are locations where the cracks may have closed in previously cracked regions. In this way, the timedependent changes in deformation and stresses are calculated, without the simplifying assumptions inherent in the AEMM, where a single time step is considered and the extent of cracking on the cross-section is assumed not to change with time.

7.5 References 1. Bischoff, P.H. (2001). Effects of shrinkage on tension stiffening and cracking in reinforced concrete. Canadian Journal of Civil Engineering, 28(3), 363–374. 2. Gilbert, R.I. and Wu, H.Q. (2009). Time-dependent stiffness of cracked reinforced concrete elements. ﬁb London 09, Concrete: 21st Century Superhero, June, London. 3. Scott, R.H. and Beeby, A.W. (2005). Long-term tension stiffening effects in concrete. ACI Structural Journal, 102(1): 31–39. 4. Bamforth, P.B. (2007). Early-age thermal crack control in concrete. CIRIA C660, London.

8

Members and structures

8.1 Introductory remarks The cross-sectional analyses developed in Chapters 4–7 form the basis for the prediction of the in-service deformation of concrete members and structures. Techniques for making such predictions are presented in this chapter. From the point of view of serviceability, it is important that the deﬂection and shortening of structural members remain acceptably small under normal in-service conditions. It is also important that crack widths are such that they do not detract from the appearance or durability of the structure. In Chapter 3, some guidance was given for the design of concrete structures for serviceability. The load combinations and design criteria for the serviceability limit states that are speciﬁed in some of the more well-known codes of practice were discussed. In this chapter, procedures for the prediction of structural behaviour at service loads for a variety of structural forms are discussed and illustrated. In most cases, reference is made to the relevant cross-sectional analyses described and illustrated in Chapters 4–7. Throughout this chapter the age-adjusted effective modulus method (AEMM) has been adopted for the analysis of the individual cross-sections, however, the member analyses could be carried out just as easily using any of the other methods of analysis introduced in Chapter 4 [such as the effective modulus method (EEM), step-by-step method (SSM) or rate of creep method (RCM)]. In Section 8.5, the effects of timedependent displacements on the behaviour of slender reinforced concrete columns at the strength limit state are also considered. Often the accurate prediction of structural behaviour at service loads is difﬁcult, particularly for many-fold indeterminate structures, but useful approximations are available to simplify many of the calculations. In the analyses presented here, approximations and simplifying assumptions are introduced from time to time to reduce the computational effort. In design, a thorough understanding of the nature and implications of these assumptions is essential if a realistic and practical interpretation of the ﬁnal results is to be made. As with all aspects of structural analysis and design, sound engineering judgment is an essential ingredient.

8.2 Deﬂection of statically determinate beams 8.2.1 Deﬂection and axial shortening of uncracked beams In Section 3.6.1, the calculation of the deﬂection and axial shortening of a member by integration of the deformations over the length of the member was discussed. If the

294 Members and structures curvature and axial strain at the centroid of the section are known at each end of a span (i.e. at cross-sections A and B in Fig. 3.1) and at mid-span (cross-section C in Fig. 3.1) and if the distributions of axial strain and curvature along the member are parabolic, the axial deformation and mid-span deﬂection of the member are given by Eqs 3.7a and b, given here and renumbered for convenience: eAB =

(εaA + 4εaC + εaB ) 6

(8.1a)

vC =

2 (κA + 10κC + κB ) 96

(8.1b)

Example 8.1 The axial shortening and mid-span deﬂection of a simply-supported, uncracked, post-tensioned concrete beam spanning 12.0 m are to be calculated, immediately after ﬁrst loading and after a period of sustained loading at time τk . An elevation of the beam is shown in Fig. 8.1, together with details of the cross-section at mid-span. The non-prestressed reinforcement is uniform along the span. The beam is post-tensioned by a single cable of parabolic proﬁle, with the depth of the tendon below the top surface of the beam (dp ) equal to 450 mm at each support and 780 mm at mid-span. The duct diameter is 70 mm. The initial tensile force in the tendon prior to transfer (at time τ0 ) is assumed to be constant along the length of the member and equal to Pp,init = 1300 kN. That is, σp,init = Pp,init /Ap = 1300 MPa at every cross-section. The prestressing duct is grouted soon after the transfer of prestress and immediately after the application of the sustained load, so that the prestressing tendon is unbonded for the short-term analysis but fully bonded to the concrete throughout the period of the time analysis. Two load cases are considered. In load case 1, the beam is subjected only to its self-weight (i.e. ws = 6.1 kN/m) plus prestress from ﬁrst loading to time τk . In load case 2, the beam carries a constant sustained uniformly distributed load of ws = 40 kN/m plus prestress from ﬁrst loading to time τk . The relevant material properties for the time period under consideration are: Ec (τ0 ) = 30,000 MPa Es = Ep = 2 × 105 MPa ϕ(τk , τ0 ) = 1.8 χ(τk , τo ) = 0.65 εsh (τk − τo ) = −400 × 10−6 and ϕp (τk , σp,init ) = 0.02 Taking the centroidal axis of the gross cross-section as the reference axis (i.e. dref = 450 mm), the initial and ﬁnal strains at the reference axis and the initial and ﬁnal curvatures are ﬁrst calculated at mid-span and at each support using the

Members and structures

295

ws 450

450

A

C

Parabolic tendon

B

6000

6000

Elevation 50

450

As(1) = 1200 mm2 450 850 780

Centroid of gross section

Agross = 254,000 mm2 Igross = 22,500 × 106 mm4 (with respect to centroidal axis)

900

Ap(1) = 1000 mm2 As(2) = 2400 mm2

Section at mid-span

Figure 8.1 Details of beam in Example 8.1 (all dimensions in mm).

cross-section analyses outlined in Sections 5.3 and 5.4. The axial deformation and deﬂection are then calculated using Eqs 8.1. For the short-term analyses, the duct is empty and the prestressing steel does not contribute to the properties of the transformed section. For the long-term analysis the duct is grouted and the prestressing steel forms part of the transformed cross-section.

Load case 1 Cross-section at mid-span The applied moment at mid-span caused by the sustained load ws = 6.1 kN/m is: Ms =

6.1 × 122 = 109.8 kNm 8

and from a cross-sectional analysis of Section 5.3, the strain at the reference axis and the curvature immediately after ﬁrst loading are εr,0 = −158 × 10−6 and κ0 = −0.411 × 10−6 mm−1 . The strain at the reference axis and the curvature at mid-span at time τk are calculated using the analysis of Section 5.4 and are equal to εr,k = −662 × 10−6 and κk = −0.641 × 10−6 mm−1 . In the time analysis, the grout was initially assumed to be unloaded. Cross-section at the supports Similar calculations for the section at each support, where Ms = 0 and dp = 450 mm, give εr,0 = −160 × 10−6 ; κ0 = 0.017 × 10−6 mm−1 ; εr,k = −690 × 10−6 ; and κk = 0.163 × 10−6 mm−1 .

296 Members and structures Axial shortening and deﬂection Using Eq. 8.1a, the axial shortening of the member is: At ﬁrst loading: ei =

12,000 (−160 − 4 × 158 − 160) × 10−6 = −1.90 mm 6

At time τk : 12,000 (−690 − 4 × 662 − 690) × 10−6 = −8.06 mm 6 The initial and ﬁnal mid-span deﬂections are found using Eq. 8.1b and are: e=

At ﬁrst loading: vci =

12,0002 [0.017 + 10 × (−0.411) + 0.017] × 10−6 96

= −6.11 mm (i.e. upward camber) At time τk : vc =

12,0002 [0.163+10×(−0.641)+0.163]×10−6 = −9.13 mm 96

Load case 2 The applied moment at mid-span caused by the sustained load ws = 40.0 kN/m is Ms = 40 × 122 /8 = 720 kNm and the strain at the reference axis and the curvature immediately after ﬁrst loading and after the period of sustained loading are εr,0 = −162 × 10−6 ; κ0 = +0.392 × 10−6 mm−1 ; εr,k = −727 × 10−6 ; and κk = +1.116 × 10−6 mm−1 . The strain and curvature at each support are the same as those calculated for load case 1, since at each support the applied moment Ms in both cases is zero. That is εr,0 = −160 × 10−6 ; κ0 = 0.017 × 10−6 mm−1 ; εr,k = −690 × 10−6 ; and κk = 0.163 × 10−6 mm−1 . Axial shortening and deﬂection The axial shortening and deﬂection of the member are obtained from Eqs 8.1a and b: At ﬁrst loading: ei = vci =

12,000 (−160 − 4 × 162 − 160) × 10−6 = −1.94 mm 6 12,0002 (0.017 + 10 × 0.392 + 0.017) × 10−6 = 5.93 mm 96

At time τk : e= vc =

12,000 (−690 − 4 × 727 − 690) × 10−6 = −8.58 mm 6 12,0002 (0.163 + 10 × 1.116 + 0.163) × 10−6 = 17.23 mm 96

Members and structures

297

The stress and strain distributions on the cross-section at mid-span are shown in Fig. 8.2 for both load cases. −373

+0.13 +0.81

+26.9

tk

ss1 = 1.3 (−81.1) t0

t0

−0.641 × 10−6 mm−1 −0.411 × 10−6 mm−1 −950 Section

tk

sp = 1300 (1099)

ss2 = −64.5 (−184) −10.28 −4.61 Stress (MPa)

−343 Strain (× 10−6) (a) Load case 1 −339

−1230

−10.2 −8.52 tk

t0 +1.109 × 10−6 mm−1 tk

Section

t0

+0.392 × 10−6 mm−1

−225 Strain (× 10−6)

ss1 = −63.8 (−235)

+14.1

sp = 1300 (1202) ss2 = −1.1 (−56.1) +0.42 +2.30 Stress (MPa)

(a) Load case 2

Figure 8.2 Stress and strain on cross-section at mid-span for Example 8.1.

8.2.2 Control of deﬂection using non-prestressed reinforcement The change in curvature on a cross-section depends on the quantity and location of the bonded reinforcement. Consider the beam analysed in Example 8.1 and shown in Fig. 8.1. By increasing the area of top steel, As(1) , on the cross-section at mid-span, the rate of change of positive curvature with time would decrease. Increased amounts of top steel are particularly effective in reducing the time-dependent increase in positive curvature when the applied load is sufﬁciently high to induce signiﬁcant compressive stresses in the top ﬁbres, such as for load case 2 in Example 8.1. An increase in top steel would therefore reduce the ﬁnal downward deﬂection of the beam in Example 8.1 (load case 2). However, when the initial curvature is negative, as for load case 1, an increased amount of top steel would cause an increase in the negative curvature with time and an increase in the upward deﬂection. By increasing the area of bottom steel, As(2) , on the cross-section at mid-span, the rate of change of positive curvature with time would increase. Increased amounts of bottom steel are particularly effective in reducing the time-dependent increase in negative curvature when the applied load on a prestressed member is small and the compressive stresses in the bottom ﬁbres are relatively high, such as for load case 1 in Example 8.1. An increase in bottom steel would therefore reduce the ﬁnal upward

298 Members and structures deﬂection of the beam for load case 1. However, when the initial curvature is positive, as for load case 2, an increased amount of bottom steel would cause an increase in the positive curvature with time and an increase in the downward deﬂection. Tables 8.1 and 8.2 show the results of several time analyses of the beam shown in Fig. 8.1 subjected to different levels of applied loading. The areas of top and bottom non-prestressed reinforcement are varied to assess the effects of steel quantity and position on the ﬁnal deﬂection. The prestressing steel details, including the cable drape and prestressing force, the cross-sectional dimensions and the material properties are as given in Example 8.1. Three different values of the sustained load are considered, namely ws = 6.1, 23.8 and 40 kN/m. When ws = 6.1 kN/m (corresponding to the self-weight of the beam only), the initial concrete stress distribution at mid-span is approximately triangular with high compressive stress at the bottom of the cross-section, decreasing to zero stress near the top of the cross-section (as determined in Example 8.1 and illustrated in Fig. 8.2a). The load level ws = 23.8 kN/m corresponds to the balanced load stage where the external load is balanced by the upward uniformly distributed load exerted on the beam by the parabolic prestressing tendon. At this balanced load stage, the initial stress distribution is uniform over the depth of each section and the initial curvature on each section is very small. When the applied load ws = 40 kN/m, the initial stress distribution at midspan is again approximately triangular with high compressive stress at the top of the section decreasing to zero near the bottom of the section (as shown in Fig. 8.2b). The moment at mid-span is therefore close to the decompression moment. From the results in Table 8.1, the effect of increasing the quantity of non-prestressed bottom reinforcement, As(2) , is to increase the restraint to creep and shrinkage deformation in the bottom of the section and thereby increase the change in positive or sagging curvature with time. The increase is most pronounced when the initial concrete compressive stress at the level of the steel is high, i.e. when the sustained applied moment is low and the section is initially subjected to a negative or hogging curvature. Increasing the quantity of bottom reinforcement therefore increases the change in downward deﬂection with time. When the beam is subjected only to its self-weight (ws = 6.1 kN/m), increasing As(2) from zero to 4800 mm2 (p = As(2) /bd = 1.25%) changes the time-dependent deﬂection from −8.55 mm (upwards) to +3.77 mm (downwards). Evidently, the inclusion of additional bottom reinforcement is an excellent way of reducing or eliminating the time-dependent upward deﬂection or camber that often causes serviceability problems in prestressed concrete construction when the sustained load is relatively light. When the beam is initially subjected to the balanced load (ws = 23.8 kN/m), increasing As(2) from zero to 4800 mm2 changes the time-dependent deﬂection from +2.90 mm (downwards) to +11.36 mm (downwards). When the sustained load is sufﬁcient to decompress the bottom ﬁbres at mid-span (ws = 40.0 kN/m), increasing As(2) from zero to 4800 mm2 changes the time-dependent deﬂection from +13.38 mm (downward) to +18.32 mm (downwards). The inclusion of tensile non-prestressed reinforcement in the bottom of a prestressed beam may increase the downward deﬂection with time and may in fact cause undesirable deﬂection in some situations. From the results in Table 8.2, the inclusion of non-prestressed reinforcement in the compressive zone, As(1) , increases the restraint to creep and shrinkage deformation in the top of the section and thereby increases the change in negative or hogging curvature with time (or reduces the change in positive curvature with time). The effect

κ0 (×10−6 mm−1 ) −0.492 −0.412 −0.350 −0.011 0.027 0.057 0.429 0.429 0.429

εr,0 (×10−6 )

−175 −158 −144

−173 −165 −158

−171 −171 −171

As(2) (mm2 )

0 2400 4800

0 2400 4800

0 2400 4800

ws (kN/m)

6.1

23.8

40.0

Initial deformation of section at mid-span

6.44 6.55 6.63

0.16 0.52 1.04

−7.38 −6.06 −5.06

Initial deﬂection at mid-span (mm)

−676 −646 −628

−655 −592 −557

−632 −534 −478

0.892 1.029 1.113

0.193 0.482 0.649

−0.570 −0.115 0.143

εr,k κk (×10−6 ) (×10−6 mm−1 )

– −46.9 −36.6

– −79.9 −59.4

– −116 −84.3

σs(2),k (MPa)

Change in deformation and steel stress with time on section at mid-span

Table 8.1 Effect of varying the area of non-prestressed tensile steel As(2) (As(1) = 0)

−108 −93.2 −84.1

−180 −144 −122

−258 −199 −164

σp,k (MPa)

13.38 16.48 18.32

2.90 8.28 11.36

−8.55 −0.68 3.77

Change in mid-span deﬂection with time (mm)

−0.412 −0.410 −0.409 0.027 −0.008 −0.036 0.429 0.360 0.306

−158 −158 −158

−165 −156 −150

−171 −155 −142

0 2400 4800

0 2400 4800

0 2400 4800

6.1

23.8

40.0

6.55 5.39 4.50

0.52 −0.12 −0.62

−6.06 −6.15 −6.22

−646 −506 −428

−592 −494 −439

−534 −481 −450

1.029 0.506 0.217

0.482 0.114 −0.094

−0.115 −0.315 −0.433

– −142 −103

– −108 −80.3

– −71.1 −55.4

−46.9 −60.8 −68.3

−79.9 −89.9 −95.3

−116 −121 −125

−93.2 −101 −106

−144 −149 −152

−199 −202 −203

σs(1),k σs(2),k σp,k (MPa) (MPa) (MPa)

Change in deformation and steel stress with time on section at mid-span

κ0 εr,0 Initial deﬂection εr,k ws As(1) κk (kN/m) (mm2 ) (×10−6 ) (×10−6 mm−1 ) at mid-span (mm) (×10−6 ) (×10−6 mm−1 )

Initial deformation of section at mid-span

Table 8.2 Effect of varying the area of non-prestressed compressive steel As(1) (As(2) = 2400 mm2 )

16.5 7.59 2.67

8.27 1.70 −1.46

−0.68 −4.73 −7.08

Change in mid-span deﬂection with time (mm)

Members and structures

301

is most pronounced when the initial concrete compressive stress at the level of the top steel is high, i.e. when the sustained applied moment is high and the section is initially subjected to a positive or sagging curvature. Increasing the quantity of top reinforcement therefore decreases the change in downward deﬂection with time. When the beam is subjected only to self-weight (ws = 6.1 kN/m), increasing As(1) from zero to 4800 mm2 (p = As(1) /bd = 1.25%) changes the time-dependent deﬂection from −0.68 mm (upwards) to −7.08 mm (upwards). The inclusion of top reinforcement therefore increases the upward camber in a prestressed concrete member with time. When the beam is initially subjected to the balanced load (ws = 23.8 kN/m), increasing As(1) from zero to 4800 mm2 changes the time-dependent deﬂection from +8.27 mm (downward) to −1.46 mm (upwards). When the sustained load is sufﬁcient to decompress the bottom ﬁbres at mid-span (ws = 40.0 kN/m), increasing As(1) from zero to 4800 mm2 reduces the time-dependent deﬂection from +16.5 mm (downward) to +2.67 mm (downwards). The inclusion of non-prestressed compressive reinforcement in the top of a reinforced or prestressed beam substantially reduces the long-term downward deﬂection. The signiﬁcant reduction with time of the resultant compressive force carried by the concrete should also be noted. In Tables 8.1 and 8.2, the time-dependent changes in the bonded steel stress on the cross-section at mid-span are reported. This gradual build up of compression in the steel at each level of bonded reinforcement is balanced by an equal and opposite tensile force acting on the concrete at that level of magnitude As(i) σs(i) or Ap σp . In Table 8.2, for example, when ws = 23.8 kN/m and when As(1) = As(2) = 2400 mm2 , the concrete on the section at mid-span is subjected to three gradually increasing tensile forces (i.e. As(1) σs(1) = 259 kN, As(2) σs(2) = 216 kN and Ap σp = 149 kN). Initially the concrete was subjected to a net compressive prestressing force of 1300 kN, but this reduces by 624 kN with time. About 48 per cent of the initial compression in the concrete is shed into the bonded reinforcement with time. The loss of prestress in the tendon is only 149 kN (11.5 per cent). Clearly, a reliable picture of the time-dependent behaviour of a partially prestressed concrete beam cannot be obtained unless the restraint provided to creep and shrinkage by the non-prestressed reinforcement is adequately accounted for. It is also evident that the presence of non-prestressed reinforcement signiﬁcantly reduces the cracking moment with time and may in fact relieve the concrete of much of its initial prestress. This increases the possibility of time-dependent cracking and the effect should be included in design considerations. Although, the restraint provided by the bonded reinforcement, generally lowers the cracking moment, a judicious placement of nonprestressed reinforcement is an effective means of controlling deﬂection and can even be used to eliminate the time-dependent change in deﬂection in situations where such changes in deﬂection are undesirable. 8.2.3 Deﬂection and axial shortening of cracked beams In Chapter 3, code-oriented methods for the prediction of deﬂection in reinforced and prestressed concrete members were presented. Where more reliable predictions of deformation are needed, more reﬁned methods of analysis may be required such as those for uncracked cross-sections, outlined in Chapters 5 and 6, and for cracked crosssections, discussed in Chapter 7. These methods of analysis may be used to predict the deﬂection of cracked members.

302 Members and structures Clearly, for a cracked member, deﬂection will be underestimated if the analysis assumes every cross-section is uncracked. On the other hand, deﬂection will be overestimated, sometimes grossly overestimated, if every cross-section is assumed to be fully cracked. Tension stiffening, or the contribution of the tensile concrete to the member stiffness, ensures that the actual deﬂection of a cracked member lies somewhere between these two extremes, i.e. between the deﬂection in the uncracked condition and in the fully-cracked condition. According to Eurocode 2 (Ref. 1), to account for tension stiffening, the average curvature at a particular cracked cross-section may be taken from Eq. 3.23 (reproduced here as Eq. 8.2): κavge = ζ κ cr + (1 − ζ )κuncr

(8.2)

where ζ is the distribution coefﬁcient presented earlier as Eq. 3.24b. The most rigorous method for determining deﬂection using the cross-sectional analyses presented in Chapters 4–7 is to calculate the cracked and uncracked curvatures at frequent cross-sections along the member and then to calculate the average curvature at each section using Eq. 8.2. For this purpose the distribution coefﬁcient ζ may be taken as:

Mcr.t 2 (8.3) ζ = 1− Ms∗ where Mcr.t is the cracking moment at the time under consideration and Ms∗ is the maximum in-service moment that has been imposed on the member at, or before, the time instant at which deﬂection is being determined. With the curvature diagram thus determined, the deﬂection can be obtained by numerical integration. If the curvatures at the critical cross-sections are calculated using Eq. 8.2, the mid-span deﬂection at the time under consideration may be conveniently obtained using Eq. 8.1b.

Example 8.2 The initial and long-term deﬂections at mid-span of a 10.4 m span simplysupported reinforced concrete T-beam are to be calculated. The beam carries a constant sustained uniformly distributed service load of 22.2 kN/m (which includes self-weight) ﬁrst applied at age τ0 . Details of the cross-section and the relevant material properties are shown in Fig. 8.3. The reinforcement is uniform throughout and shrinkage is assumed to commence at τ0 . The cross-section is the same as that shown in Fig. 7.6 and analysed in Examples 7.1 and 7.3. The = 0.6 f = 3.0 MPa, ﬂexural tensile strength of the concrete is taken to be fct.f c , cracking is deemed to have so wherever the extreme ﬁbre stress exceeds fct.f occurred. The bending moment diagram for the simply-supported span is illustrated in Fig 8.4a. From a short-term analysis of the uncracked cross-section, the stress = 3.0 MPa when the applied moment in the bottom concrete ﬁbres reaches fct.f is 149.3 kNm, i.e. at points D and D’ in Fig. 8.4a, 1.514 m from each support. It is evident that, within 1.514 m from each support, the member is initially uncracked, whilst further into the span cracking occurs.

Members and structures

303

1000

f ′c = 25 MPa

100

Ec = 25,000 MPa

322

x

Es = 200,000 MPa

530

f(tk ,t0) = 3.0

y

c(tk ,t0) = 0.65

As = 4000 mm2

70

esh(tk − t0) = −500 × 10−6

400

Figure 8.3 Cross-sectional details and material properties for Example 8.2 (dimensions in mm).

Using the cross-sectional analyses of Sections 5.3 (short-term) and 5.4 (timedependent) for the uncracked portions of the span and Sections 7.2 (short-term) and 7.3 (time-dependent) for each fully-cracked cross-section, the initial and ﬁnal curvatures at any cross-section along the member may be calculated. It is noted that shrinkage causes an increase in the bottom ﬁbre tensile stress in the concrete on the uncracked cross-sections, effectively reducing the cracking moment from 149.3 kNm to 56.4 kNm with time. The extent of cracking therefore increases with time until eventually only 0.514 m at each end of the span remains uncracked. In Fig. 8.4b, the portion of the curvature diagram at time τk between points E and D on the span is approximated as a straight line. 10.4 m 1.514 m 0.514 m A 56.4 B

E

C

D

D′

149.3

300

(a) Bending moment (kNm) 1.514 m

0.521 × 10−6 0.885 × 10−6

0.318 × 10−6 0.718 × 10−6 1.442 × 10−6

2.053 × 10−6

At t0 3.237 × 10−6

At tk

(b) Curvature (mm−1) Figure 8.4 Bending moment and curvature diagrams of Example 8.2.

304 Members and structures Plots of the initial and ﬁnal curvatures are made in Fig 8.4b and a summary of the calculated curvatures at various points along the beam is made in Table 8.3. Table 8.3 Initial and ﬁnal curvatures in beam of Example 8.2 At time τ0

At time τk

Distance from support, z (mm)

Moment (kNm)

Curvature (mm−1 )

Moment (kNm)

Curvature (mm−1 )

0 0.514 1.514 − 1.514 + 3.075 5.2

0 56.4 149.3 149.3 250.0 300.0

0 0.120 × 10−6 0.318 × 10−6 0.718 × 10−6 1.202 × 10−6 1.442 × 10−6

0 56.4 149.3 149.3 250.0 300.0

0.521 × 10−6 0.885 × 10−6 2.053 × 10−6 2.053 × 10−6 2.841 × 10−6 3.237 × 10−6

The initial mid-span deﬂection of the cracked member at ﬁrst loading τ0 and the ﬁnal deﬂection at time τk calculated by numerically integrating these curvature diagrams are: (vc )cr.0 = 15.98 mm and (vc )cr.k = 38.14 mm. A close approximation of these more accurate (but considerably more tedious) calculations may be obtained using Eq. 8.1b (viz., (vc )cr.0 = 16.25 mm and (vc )cr.k = 37.64 mm). If cracking was ignored and the curvature diagrams were calculated based on the uncracked section properties, the mid-span deﬂection at times τ0 and τk would be (vc )uncr.0. = 7.19 mm and (vc )uncr.k = 28.03 mm. At time τ0 and τk , Eq. 8.3 gives: ζ0 = 1 −

149.3 300

2 = 0.752 and ζk = 1 −

56.4 300

2 = 0.965

and using the following expressions (similar to Eq. 8.2), the ﬁnal mid-span deﬂections of the cracked member accounting for tension stiffening at ﬁrst loading and at time τk are: vc.0 = ζ (vc )cr.0 + (1 − ζ )(vc )uncr.0 = 0.752 × 15.98 + (1 − 0.752) × 7.19 = 13.8 mm vc.k = ζ (vc )cr.k + (1 − ζ )(vc )uncr.k = 0.965 × 38.14 + (1 − 0.965)×28.03=37.8 mm

For most practical purposes, knowledge of the curvature at each end of a member and at mid-span at any particular time after ﬁrst loading is generally sufﬁcient to make a reliable estimate of the deﬂection of a cracked reinforced concrete member.

Members and structures

305

8.3 Statically indeterminate beams and slabs 8.3.1 Discussion In each cross-sectional analyses presented in Chapters 4–7, the internal actions were known and the changes in strain and curvature on a particular cross-section were assumed to occur without restraint from either the supports or adjacent parts of the structure. While this assumption is perfectly reasonable for statically determinate members, it may be unreasonable for continuous members. Consider a plain concrete continuous beam subjected to a uniformly distributed load that is small enough to avoid cracking. If the concrete is assumed to be homogeneous, with the same creep characteristics throughout, the effect of creep is simply to reduce the effective modulus and to increase the strains and displacements with time. There is no change in the reactions at the supports and consequently no change in the internal actions on any cross-section. However, if the creep characteristics are not uniform throughout, creep will induce reactions at the supports and cause a change in the distribution of internal actions. In practical concrete structures, the creep characteristics are rarely uniform. Different parts of a structure may have different ages and therefore different creep coefﬁcients. If part of a structure has cracked, its response to creep is different from that of the uncracked parts of the structure. In addition, the quantity of reinforcement may vary from region to region and therefore the amount of internal restraint to creep will vary accordingly. Therefore, in statically indeterminate concrete structures, creep may lead to a considerable redistribution of internal actions with time. Shrinkage also may cause signiﬁcant changes in the distribution of internal actions with time in indeterminate members. If a member is not free to shorten, shrinkage produces internal tension. Shrinkage-induced curvature on each cross-section due to the restraint provided by asymmetrically placed steel reinforcement can introduce signiﬁcant reactions at the supports and hence signiﬁcant changes in the internal actions on each cross-section. Consider the uncracked, propped cantilevers shown in Fig. 8.5. The member in Fig. 8.5a(i) contains a preponderance of reinforcement in the bottom ﬁbres and shrinkage causes a positive curvature in the singly reinforced region. If the weight of the beam and any applied loads are ignored and if the support at B is removed, shrinkage would cause the member to gradually deﬂect upwards, as indicated. With the support at B, in fact, resisting upward movement, a downward reaction RB.k gradually develops with time, as shown. The initial reaction at B caused by the load on the beam RB.0 is therefore reduced by RB.k and this leads to an increase in the negative moment at support A and a decrease in the positive moment at mid-span. Shrinkage therefore causes the time-dependent redistribution of moments shown in Fig. 8.5b(i). Note that the shrinkage-induced reactions at the built-in support at A (namely, a vertical reaction RA.k , equal and opposite to RB.k , and a moment MA.k = RB.k L) are not shown in Fig. 8.5. For the member shown in Fig. 8.5a(ii), with a preponderance of steel in the top, shrinkage causes an upward reaction RB.k to develop with time at support B. As a consequence, the positive span moments increase with time and the negative moment at support A decreases, as shown in Fig. 8.5b(ii).

306 Members and structures −ve ksh

+ve ksh

Straight

Straight

As A (i)

As B

As

ΔRB.k

L

A (ii)

B

As L

DRB.k

(a) Unrestrained shrinkage deformation and shrinkage–induced reaction at support B Applied load

A

Applied load

B

A

B

RB.0

RB.0 RB.0 + DRB.k

RB.0 + DRB.k First loading, t0 Time tk after shrinkage

(i)

First loading, t0 Time tk after shrinkage

(ii) (b) Redistribution of bending moments caused by shrinkage

Figure 8.5 Effects of shrinkage in a one-fold indeterminate beam.

Of course, the shrinkage-induced actions occur gradually and are therefore relieved by creep. If shrinkage were not accompanied by creep, the time-dependent redistribution of internal actions would be signiﬁcantly greater than it actually is. 8.3.2 Determination of redundants A detailed discussion of the various techniques commonly employed for the analysis of statically indeterminate structures is not attempted here. There are numerous excellent texts on structural analysis, including Refs 2 and 3. In this section, a brief revision of the force method of structural analysis is made and the way in which the method can be used for the time-analysis of indeterminate structures is described and illustrated by example. In the following, the structure is initially assumed to be homogeneous. In the force method, a n-fold indeterminate structure is converted into a statically determinate primary structure by the selection of n internal actions (or external reactions) as redundants and making the corresponding releases. Let the vector of redundant forces be RR . The vector of external loads P applied to the primary structure produces reactions RP at the supports and the external loads (or the load-independent environmental effects such as temperature change or shrinkage) cause displacements of the primary structure at each release uP . These displacements are incompatible with the support

Members and structures

307

conditions of the indeterminate structure and must be eliminated by the unknown redundant forces. If the primary structure is subjected to a unit virtual force at the position of the ˜ Ri = 1, the resulting displacements at each of the n releases are i-th redundant, i.e. R called ﬂexibility coefﬁcients and are denoted fi1 , fi2 , … fin . If ﬂexibility coefﬁcients are determined for unit values of each redundant, an n × n ﬂexibility matrix F may be established, where the term fij is the displacement of the primary structure at release j due to a unit value of the ith redundant. The reactions at the supports of the primary structure caused by unit values of the redundants are also calculated and may be assembled into an m by n matrix RPR where m is the number of reactions in the primary structure. The redundant forces are obtained by solving the following set of simultaneous equations which is generated when compatibility is enforced at each release: F RR = −uP

(8.4)

where, if necessary, support movements could also be included on the right hand side of the equation. The reactions of the statically indeterminate structure are obtained by adding the reactions caused by the redundants (RPR RR ) to the reactions calculated earlier for the released structure RP . That is: R = RP + RPR RR

(8.5)

For a structure with uniform creep characteristics throughout that is subjected to constant sustained loads, the deformation at time τk will be (1 + ϕ) times the deformation at ﬁrst loading τ0 , where ϕ (= ϕ(τk , τ0 )) is the creep coefﬁcient at time, τk , due to a stress ﬁrst applied at τ0 . If the presence of the reinforcement is ignored and if cracking is also ignored, the displacements u at time τk are (1 + ϕ) times their value at τ0 and each term of the ﬂexibility matrix F is also increased by the factor (1 + ϕ). In addition, the reactions R of the statically indeterminate structure do not change and therefore there is no change in the internal actions with time. As has been previously pointed out, this not the case, however, in most concrete structures where the reinforcement layout varies throughout the structure and the extent of cracking also varies. The propped cantilevers shown in Fig. 8.5a are a typical case. The reinforcement is not uniform throughout and, in all probability, parts of the beams are cracked and parts are not. The creep characteristics are therefore far from uniform. In such structures, some creep-induced change in the reactions (and in the internal actions) with time can be expected. In Section 8.3.1, the change in reactions of the members shown in Fig. 8.5a caused by shrinkage warping was also discussed. To calculate the time-dependent change in reactions and internal actions during any time interval (τk – τ0 ), it is ﬁrst necessary to calculate the change in the displacements of the primary structure at each release, uP . The displacements caused by both creep and shrinkage are included here, plus any other displacement that may occur during the time interval, perhaps due to support settlement, additional external loads, losses of prestress, and so on. The AEMM may be used to include time-dependent deformations and an ageadjusted ﬂexibility matrix F can also be determined. Changes in the redundants with time are developed gradually between τ0 and τk and the creep plus elastic displacements

308 Members and structures caused by these gradually applied redundants forces may be calculated using the age-adjusted modulus for concrete Ee (deﬁned in Eq. 4.35) instead of Ec . The ageadjusted ﬂexibility matrix F is therefore formed in exactly the same way as F, except that the displacement (elastic + creep) at each release due to the gradually applied unit force at the position of the ith redundant is calculated using Ee . The time-dependent change in the redundants is obtained by solving the compatibility equations: FRR = −uP

(8.6)

and the change in the reactions of the statically indeterminate structure are: R = RP + RPR RR

(8.7)

where RP is the change in reactions of the primary structure due to any changes of the external loads during the time interval under consideration. For the analysis of a statically indeterminate reinforced or prestressed concrete beam or frame, the procedures outlined in Chapters 4–7 may be used to calculate the deformation (strain and curvature, εr.k and κk ) on any cross-section of the determinate primary frame at any time. When deformations have been determined at several sections, the time-dependent changes in displacement u may be calculated by numerical integration or by virtual work. In this way, the effect of the reinforcement and the inﬂuence of cracking, as well as the effects of creep and shrinkage, can be included directly in the time analysis of an indeterminate member.

Example 8.3 The ﬁnal shrinkage-induced internal actions at time τk in the unloaded and uncracked propped cantilever shown in Fig 8.6 are to be determined. The structure is, of course, one-fold indeterminate, that is, n = 1. Ec = 25,000 MPa; ϕ = 2.5; χ = 0.65; ∗ = −600 × 10−6 ; and E = Ec = 9,524 MPa. εsh e 1+χϕ 300

300

As

A

50

As = 1860 mm2 3000 Region 1

7000 Region 2 Elevation

B

As = 1860 mm2 Region 2

550

500

50

50 Region 1

Sections

Figure 8.6 Dimensions and properties of the beam in Example 8.3 (all dimensions in mm).

Using the procedures outlined in Section 5.4, the age-adjusted effective modulus is used to determine the ﬁnal shrinkage-induced curvature on an

Members and structures

309

otherwise unloaded and unrestrained cross-section in Region 2: (κsh )2 = 0.663 × 10−6 mm−1 . The shrinkage-induced curvature in Region 1 is zero, because each cross-section is symmetrically reinforced (and uncracked). The vertical reaction at support B is selected as the redundant, i.e. RR = VB . The primary structure is therefore a cantilever ﬁxed at support A. The change in the vertical displacement of the primary structure at support B (uB ), due to the shrinkage-induced curvature distribution shown in Fig. 8.7a, is calculated using the second moment area method as: uB =

0.663 × 10−6 × 70002 = 16.24 mm 2 0.663 × 10−6 mm−1 DuB B

A 3000 Region 1

A

B

7000 Region 2

(a) Shrinkage curvature

(b) Deflected shape

Figure 8.7 Shrinkage-induced curvature and deﬂected shape of primary structure in Example 8.3.

The vertical displacement at B due to a gradually applied unit force at B is f11 and is obtained from the curvature diagram shown in Fig. 8.8c, calculated by analysing the uncracked section in the various regions of the cantilever: f11 = 0.1301 × 10−6 ×

10,0002 70002 + (0.1299 − 0.0911) × 10−6 × 3 3

= 4.97 mm/kN B A

10 m

1 kN

(a) Unit load at B

+10

(b) Moment, M (kNm) +0.0911 +0.1301

+0.1299

(c) Curvature (10−6mm−1) f11 (d) Deflected shape

Figure 8.8 Virtual moment and curvature diagram in Example 8.3.

310 Members and structures The redundant VB is calculated from Eq. 8.6 as: f¯11 VB = −uB

from which

VB =

−16.24 = −3.27 kN (i.e. ↓) 4.97

The shrinkage-induced internal actions and external reactions are shown in Fig. 8.9. −32.7 kNm

32.7 kNm A

B

3.27 kN

−3.27 kN

3.27 kN (a) Reactions

(b) BMD

(c) SFD

Figure 8.9 Shrinkage-induced reactions, bending moment and shear force diagrams for Example 8.3.

Example 8.4 The reactions of the one-fold indeterminate propped cantilever of Fig. 8.6 are to be determined at times τ0 and τk . A uniformly distributed load ws = 8 kN/m ﬁrst applied at τ0 is assumed to remain constant with time. The material properties are as for Example 8.3 and the ﬂexural tensile strength of concrete is taken to = 3.0 MPa. be fct.f

1. Calculation of the reactions at time τ0 immediately after the application of w s (a) Ignoring the effects of cracking As in the previous example, the vertical reaction at support B is selected as the redundant, i.e. RR = VB . The 8 kN/m uniformly distributed load produces the following reactions at support A of the primary beam: MA = −400 kNm and VA = 80 kN, therefore:

RP =

−400 MA = 80 VA

If the ﬂexural rigidity EI (= M/κ) is constant throughout the entire span, the vertical displacement at the end of the cantilever at B due to a uniform load ws is: uB = −

ws L4 8EI

Members and structures

311

and the vertical displacement at B due to a unit vertical (upward) force at B (f11 ) and the corresponding reactions of the primary structure are: f11 =

L3 3EI

and

RPR =

MA = L VA = −1

From Eq. 8.4: VB ×

L3 wL4 = 3EI 8EI

and therefore VB =

3wL = 30 kN(↑) 8

The other reactions of the statically indeterminate frame are obtained from Eq. 8.5: ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ MA −400 10 −100 kN.m ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ R = ⎣ VA ⎦ = ⎣ +80 ⎦ + ⎣ −1 ⎦ × 30 = ⎣ +50 kN ⎦ 0 1 +30 kN VB If the effects of cracking are ignored, the bending moment diagram of the indeterminate member immediately after ﬁrst loading is shown in Fig. 8.10. MA = −100.0 5m 3.75 m

− C

A

B +

50.0

56.25

Figure 8.10 Initial bending moment diagram (ignoring cracking) in kNm for Example 8.4.

If the effects of cracking are also ignored in the calculation of deﬂection (which, of course may grossly underestimate the actual deﬂection), the initial curvature on the doubly-reinforced section at support A and on the singly-reinforced section at the mid-span C are calculated using the analysis outlined in Section 5.3 as κA,0 = −0.569 × 10−6 mm−1 and κC,0 = +0.325 × 10−6 mm−1 , respectively. The short-term deﬂection at mid-span vC may be determined using Eq. 8.1b: vC =

10,0002 [−0.569 + 10 × 0.325 + 0] × 10−6 = 2.79 mm 96

312 Members and structures (b) Including the effects of cracking From a short-term cross-sectional analysis of the singly reinforced section in the positive moment region (Region 2), the cracking moment is 65.3 kNm. This is greater than the maximum positive moment in Fig. 8.10 and, therefore, the midspan region is not cracked initially. For the doubly reinforced section at support A (in Region 1), the cracking moment is 70.3 kNm. Therefore, the beam is cracked in the negative moment region near support A. The previous analysis must now be modiﬁed to include the effects of cracking at A. Tension stiffening is not considered here, but could be easily taken into account using the averaging procedure discussed in Section 8.2.3. If the bending moment diagram in Fig. 8.10 is taken as an initial approximation, the extent of cracking is small, with the cracked region extending just 0.625 m from support A. The curvatures at sections in the various regions of the beam are calculated from short-term cross-sectional analyses (Section 5.3 for the uncracked cross-sections and Section 7.2 for the cracked cross-sections) and the instantaneous ﬂexural rigidities (EI = M/κ) are: In Region 1: In Region 2:

Uncracked

(EI)cr.1 = 70.67 × 1012 Nmm2 (EI)uncr.1 = 175.7 × 1012 Nmm2

Uncracked

(EI)uncr.2 = 154.0 × 1012 Nmm2

Cracked

As previously calculated:

−400 MA RP = = +80 VA and the vertical displacement at the end of the primary beam (at B) due to ws = 8 kN/m is found, by moment-area methods or by virtual work, from the curvature diagram shown in Fig. 8.11a and equals uB = −78.5 mm. The displacement at B of the cracked member due to a unit vertical force at B is found from the curvature diagram in Fig. 8.11b and equals f11 = 2.51 mm/kN. From Eq. 8.4: VB =

−uB 78.5 = = 31.3 kN(↑) f11 2.51

and the reactions of the statically indeterminate beam are obtained from Eq. 8.5: ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ −400 10 −87 kN.m MA ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ {R} = ⎣ VA ⎦ = ⎣ 80 ⎦ + ⎣ −1 ⎦ × 31.3 = ⎣ 48.7 kN ⎦ 0 1 31.3 kN VB The bending moment and curvature diagrams after cracking are illustrated in Fig. 8.12. The short-term deﬂection at mid-span may be obtained by virtual work from the curvature diagram in Fig. 8.12 and is vc = 3.17 mm. For this beam, cracking at, and near, the support at A causes a reduction in the negative moment at A, an increase in the positive span moments and a 14 per cent increase in mid-span deﬂection. After initial cracking, moment is shed to the stiffer uncracked parts of the structure. If the load w was increased,

Members and structures

313

w = 8 kN/m A

B

B

A

10 m −400

1 kN

−351.6 −196

A

B 0.625 m 3m 7m Moment (kNm)

−5.66 ×

10−6

+10 Moment (kNm)

−4.975 × 10−6 −2.001 × 10−6 −1.273 × 10−6

+0.0398 × 10−6

−1.116 × 10−6 A

+0.0534 × 10−6

B Curvature (M/EI) (mm−1)

0.1415 ×

(a) Moment and curvature caused by w

10−6

+0.0455 × 10−6

+0.1327 × 10−6 Curvature (M/EI) (mm−1) (b) Moment and curvature caused by a unit load at B

Figure 8.11 Moment and curvature diagrams for cracked primary beam of Example 8.4. 0.625 m

7.0 m

2.375 m

−1.238 × 10−6

MA = −87.5

−58.5 −

5m 3.908 m C

A 22.8

B +

56.3

61.1

(a) Bending moment diagram (kNm)

−0.828 × 10−6

− −0.333 × 10−6 C A 0.130 × 10−6 0.148 × 10−6 0.366 × 10−6

B +

0.397 × 10−6

(b) Curvature diagram (mm−1)

Figure 8.12 Moment and curvature diagrams after cracking in Example 8.4.

cracking would also occur in the positive moment region. With the member more uniformly cracked and the stiffness more uniform in the peak moment regions, the bending moments would redistribute back towards the distribution shown in Fig. 8.10, but the deﬂection would increase signiﬁcantly due to the reduction in the ﬂexural rigidity for Region 2 from (EI)uncr.2 to (EI)cr.2 .

2. Calculation of the reactions at time τk after creep and shrinkage Let the change in reaction at support B be the unknown redundant at time τk , i.e. RR = VB.k . The primary structure (cantilevered beam) is shown in Fig. 8.13a, together with the external loads and the known reactions immediately after ﬁrst

314 Members and structures loading (at τ0 ). Using the procedures outlined in Sections 5.4 and 7.3 for the time analysis of the uncracked and fully-cracked cross-sections, respectively, the curvature diagram at τk after creep and shrinkage is calculated and illustrated in Fig. 8.13b and the curvature diagram due to creep (with shrinkage set to zero) is shown in Fig. 8.13c. The creep and shrinkage characteristics of the concrete are those of Example 8.3 and given in Fig. 8.6. Although not strictly correct, the extent of cracking is assumed to remain unchanged with time. Of course, at ﬁrst loading, the deﬂection of the primary beam at B is zero. But as the primary beam creeps and shrinks under the constant sustained loads shown in Fig. 8.13a, the deﬂection at B becomes non-zero. By numerical integration of the curvature diagrams at time τk (in Fig. 8.13b and c), the deﬂection of the primary cantilever at B is uB = 20.5 mm (upwards) when both creep and shrinkage are considered and uB = 8.49 mm for creep only. −2.153 × 10−6 MA = −87.4 kNm

−0.761 × 10−6

8 kN/m 10 m VB = 31.3 kN

VA = 48.7 kN

3.908 m

0.297 × 10−6 1.086 × 10−6

+0.663 × 10−6

1.796 × 10−6 (b) Curvature of primary beam (mm−1) – creep and shrinkage

(a) Loads on primary beam −1.548 × 10−6

−1.640 × 10−6

−1.029 × 10−6 −0.761 × 10−6

0.297 × 10−6 0.429 × 10−6

3.908 m

1.136 × 10−6

(c) Curvature of primary beam (mm−1) – creep only

Figure 8.13 Load and curvature diagrams of released structure in Example 8.4.

The vertical displacement at the end of the cantilever (at B) at time τk due to a gradually applied unit force at B is f11 and may be calculated by ﬁrst analysing the various cross-sections to determine the long-term curvature. The ﬁnal curvature diagram associated with a unit virtual force at B is shown in Fig. 8.14. A

B

0.625 m

f11

0.1220 × 10−6

+1 +10.0

Loads

2.375 m

0.1771 × 10

Moments

−6

7.0 m

0.0911 × 10−6

0.1299 × 10−6 0.1660 × 10−6

Curvature (mm−1)

Figure 8.14 Moment and curvature at time τk due to gradually applied unit virtual load at B in Example 8.4.

Members and structures

315

The deﬂection at B due to a unit virtual force at B (f11 ) is readily obtained from the curvature diagram using moment-area methods or numerical integration: f11 = 0.1299 ×

7.02 + 0.0911 × 2.375 × 8.188 + (0.1220 − 0.0911) 3

2.375 × 8.583 + 0.1660 × 0.625 × 9.688 + (0.1771 − 0.1660) 2 0.625 × × 9.792 = 5.25 mm/kN 2

×

From Eq. 8.6, the change in the reaction at B with time is: VB = −

uB 20.5 =− = −3.90 kN(i.e. ↓)− for both creep and shrinkage ¯f11 5.25

VB = −

8.49 = −1.62 kN(i.e. ↓)− for creep only 5.25

In Fig. 8.15, the reactions at time τk and the corresponding internal actions are compared with the values immediately after ﬁrst loading. Note that although the MA = −87.4 kNm

MA = −126.0 kNm

8 kN/m 10 m

8 kN/m 10 m

VB = 31.3 kN

VA = 48.7 kN

VA = 52.6 kN Final reactions (at tk)

Initial reactions (at t0)

VB = 27.4 kN

−126.0 kNm

−87.4 kNm

+ 46.9 kNm

+ 61.1 kNm Initial bending moments (at t0)

Final bending moments (at tk)

(a) Initial actions (at t0)

(b) Final actions (at tk) – creep + shrinkage

MA = −103.5 kNm

8 kN/m 10 m VB = 29.7 kN

VA = 50.3 kN Final reactions (at tk) −103.5 kNm

+ 54.9 kNm Final bending moments (at tk) (b) Final actions (at tk) – creep only

Figure 8.15 Initial and ﬁnal reactions and moments in Example 8.4.

316 Members and structures initial cracking at A caused a reduction in the peak negative moment at the ﬁxed support, the effect of creep and shrinkage is to substantially increase the moment at support A and reduce the positive moment at mid-span. In this example, creep causes the magnitude of the moment at A to increase by about 18 per cent (from 87.4 to 103.5 kNm) and shrinkage causes a further increase of 26 per cent (from 103.5 to 126.0 kNm). In the positive moment region, shrinkage-induced tension in the concrete may cause time-dependent cracking and this will reduce the stiffness of the positive moment region resulting in a further increase in the negative support moment and a decrease in the positive span moments. The increase in negative moments will increase the extent of cracking near the support and this, in turn, will cause a slight redistribution of moments from the negative to the positive moment region.

8.3.3 Effects of deformation or settlement at the supports If a statically indeterminate member is subjected to a sudden movement of the supports, changes in the magnitudes of the reactions and internal actions occur. If the imposed deformation at the supports is kept constant, the reactions and internal actions gradually change with time due to relaxation. If the support deformations occur gradually, the changes in reactions and internal actions also occur gradually. The simultaneous development of creep causes a relaxation of the internal forces as the support movements are taking place. Therefore, the reactions induced in an indeterminate member by a gradual deformation at one or more supports tend to increase from zero (at the commencement of movement) to a maximum value as the maximum deformation is approached, and then reduce as creep continues after the support deformation has ceased. Consider the propped cantilever beam AB subjected to a sudden support settlement δB (τ0 ) at time τ0 , as shown in Fig. 8.16. The time-dependent reactions introduced at the supports are also shown. Immediately after the support settlement at time τ0 , the vertical reaction at B can be determined using the force method. For a beam with uniform cross-section throughout: RB (τ0 ) =

3Ec I δB (τ0 ) L3

(8.8)

where I is the second moment of area of the transformed section about its centroidal axis. The change in the reaction at support B that occurs with time over the time period τk − τ0 is: RB = RB (τk ) − RB (τ0 ) MA(t)

(8.9)

A

B dB(t0)

RA(t) L

RB(t)

Figure 8.16 Time-dependent reactions caused by a support settlement.

Members and structures

317

and may be determined using the procedure outlined in Section 8.3.2 (and Eqs 8.6 and 8.7). If the support settlement δB (t) is gradually applied, the reaction RB (t) increases gradually with time. If the settlement occurs at the same rate as the creep of the concrete, the reaction at B in a member of uniform cross-section may be approximated by: RB (t) =

3Ee I¯ δB (t) L3

(8.10)

where I is the second moment of area of the age-adjusted transformed cross-section about its centroidal axis. After the support settlement reaches its maximum value at some time τ1 , the subsequent change in the reaction with time (at t > τ1 ), RB = RB (t) − RB (τ1 ), may be calculated using Eq. 8.6.

Example 8.5 The initial and ﬁnal internal actions in the unloaded and uncracked member shown in Fig. 8.17 are to be determined, if the support at B suffers a vertical displacement of 20 mm, as shown. 300

MA(t)

A

B 20 mm

50

As = 1860 mm2

500 RA(t)

RB(t)

As = 1860 mm2

50

10 m Elevation

Cross-section

Figure 8.17 Details of beam subjected to support settlement in Example 8.5.

(a) If the support settlement occurs suddenly at 28 days Maternal and cross-sectional properties are Ec (τ0 ) = 25,000 MPa; I = 7028 × 106 mm4 ; ϕ(∞, τ0 ) = 2.8; χ (∞, τ0 ) = 0.65. The reaction at B at age τ0 , immediately after the support displacement, is found using Eq. 8.8: RB (τ0 ) =

3 × 25,000 × 7028 × 106 × 20 = 10.54 kN ↓ 10,0003

and the internal bending moment varies from zero at B to −105.4 kNm at A. The initial curvature varies from zero at B to κA.0 = MA /Ec I = −0.60 × 10−6 mm−1 at A as shown in Fig. 8.18b. It is assumed here that the member remains uncracked throughout. The ﬁnal curvature at end A, caused by the sustained

318 Members and structures moment of −105.4 kNm, is calculated using the cross-sectional analysis of Section 5.4 and equals κA.k = −1.434 × 10−6 mm−1 , as shown in Fig 8.18b. The creep-induced change of curvature at end A is therefore κA.k − κA.0 = −0.834 × 10−6 mm−1 . If the displaced beam is released at B, the creep induced curvature causes a gradual displacement at end B given by: 0.834 × 10−6 × 10,0002 = 27.8 mm ↓ 3

uB =

For this member, the age-adjusted effective modulus is Ee = 8865 MPa and the second moment of area of the age-adjusted transformed cross-section about its centroidal axis is I = 10,410 × 106 mm4 . The vertical displacement caused by a gradually applied unit load (1 kN) at B is: f11 =

L3 3Ee I

=

10,0003 = 3.61 × 10−3 mm/N 3 × 8865 × 10,410 × 106

and the change in the reaction at B with time is: RB =

uB f 11

=

27.8 = 7701 N = 7.70 kN ↑ 3.61 × 10−3

The ﬁnal reaction at B is therefore: RB (τk ) = RB (τ0 ) + RB = 10.54 − 7.70 = 2.84 kN(↓) and the moment at A relaxes from −105.4 kNm at τ0 to a ﬁnal value of −28.4 kNm.

MA(t) = 105.4 kNm A

B

−0.834 20 mm

Creep induced initial

−0.600

RB(t0) =10.54 kN

RB(t0) = 10.54 kN 10 m

(b) Initial and final curvature of released structure (×10−6 mm−1)

(a) Initial reactions due to 20 mm support settlement 20 mm DuB

(c) Final deformation of released structure

Figure 8.18 Actions and deformations of released primary beam in Example 8.5.

Members and structures

319

(b) If support settlement of 20 mm occurs gradually between τ0 = 28 days and τ1 = 180 days It is here assumed that the rate of settlement is similar to the rate of creep and the following material properties are assumed: For concrete loaded at 28 days: Ec (28) = 25,000 MPa; ϕ(180, 28) = 1.5; ϕ(∞, 28) = 2.8; χ(180, 28) = χ (∞, 28) = 0.65 For concrete loaded at 180 days: Ec (180) = 30,000 MPa; ϕ(∞, 180) = 1.0; χ (∞, 180) = 0.65. The age-adjusted effective modulus at age 180 days due to a stress ﬁrst applied at 28 days is Ee = 12,660 MPa and the second moment of area of the corresponding age-adjusted transformed cross-section is I = 8841 × 106 mm4 . The reaction at B at τ1 = 180 days, when δB reaches 20 mm, is calculated using Eq. 8.10: RB (180) =

3 × 12,660 × 8841 × 106 × 20 = 6720 N = 6.72 kN(↓) 10,0003

and the corresponding moment at the ﬁxed support A is −67.2 kNm. If the displacement at B remains constant at 20 mm after τ1 = 180 days, the reactions and internal actions will gradually decrease, in the same manner as in case (a). The change in reaction at B that occurs after τ1 , RB , is selected as the redundant. The creep-induced curvature κA that develops at A in the primary beam due to a sustained moment of −67.2 kNm (after t = 180 days) is calculated using the cross-sectional analysis presented in Section 5.4. With ϕ(∞, 180) = 1.0 and χ (∞, 180) = 0.65, κA is equal to −0.223 × 10−6 mm−1 . The resulting timedependent change in deﬂection of the primary beam at B is: uB =

−0.223 × 10−6 × 10,0002 = −7.43 mm (i.e. ↓) 3

The appropriate properties of the age-adjusted transformed section are Ee = 18,180 MPa and I = 7725 × 106 mm4 . Due to a gradually applied unit load at B: f11 =

10,0003 = 2.37 × 10−3 mm/N 3 × 18,180 × 7725 × 106

The change in the reaction at B, which occurs after τ1 = 180 days, is therefore: RB = −

−7.43 = 3140 N = 3.14 kN(↑) 2.37 × 10−3

and the ﬁnal reaction at B is therefore RB (∞) = 6.72 − 3.14 = 3.58 kN (↓). The corresponding bending moment at the ﬁxed end of the member MA (∞) = −35.8 kNm.

320 Members and structures

Bending moment at support A MA (kNm)

Plots of MA versus time for both the sudden support settlement and the gradual support settlement are shown in Fig. 8.19.

100 (a) Sudden support settlement 80 60 40 (b) Gradual support settlement

20

Time, t 0 28

180

Figure 8.19 Time variation of moment due to sudden and gradual support settlement in Example 8.5.

8.3.4 Further effects of creep in prestressed construction Although creep in continuous members causes a dramatic reduction of the internal actions caused by imposed deformation (as shown in curve (a) of Fig. 8.19), the effects of creep on the redistribution of internal actions in continuous members subjected to imposed loads is less pronounced, but still signiﬁcant (as demonstrated in Example 8.4). In general, internal actions are redistributed from the regions with a higher creep rate to the regions with the lower creep rate. In Example 8.4, with the rate of change of curvature due to creep in the singly-reinforced mid-span Region 2 greater than the rate of change of curvature in the doubly-reinforced Region 1, creep causes a decrease in the positive span moments with time and an increase in the negative moments at the continuous support (see Fig. 8.15). The internal actions caused by prestress are also affected by creep of concrete. They are obviously affected by the losses of prestress caused by creep and these losses can vary from near zero, when the member is cracked at the level of the tendon, to as much as 20 per cent or more, when the member is heavily prestressed at an early age and the concrete compressive stress at the level of the bonded tendon is high. The hyperstatic reactions induced by prestress in indeterminate structures are in fact imposed loads applied to the structure at the supports and the resulting secondary moments are affected by creep. If the structural system changes after the application of some of the prestress, creep may cause a change in the hyperstatic reactions. As an example, consider the two-span beam shown in Fig. 8.20. The beam is fabricated by erecting two simply-supported prismatic precast concrete girders (of constant cross-section) over the two spans of length L. Each girder contains a single layer of straight pretensioned strands at a

Members and structures

321

In-situ joint e

A

B Pretensioning tendon L

C Precast, pretensioned girder L

Figure 8.20 Providing continuity at a continuous support.

constant eccentricity e below the centroidal axis of the cross-section. The structure is then rendered continuous by casting an in-situ joint over the interior support. Any time-dependent defomations in the members will be restrained by the imposed ﬁxity at the interior support and hyperstatic reactions will develop with time, together with the associated secondary moments and shears. Before the in-situ joint in Fig. 8.20 is cast, the two-precast girders are simply supported, with zero deﬂection but some non-zero slope at the interior support at B. Immediately after the joint is fabricated and continuity is established, the internal primary moment imposed by the prestress on each cross-section is Pe about the centroidal axis, but the initial secondary moment at B (and elsewhere) is zero. With time, creep will cause a gradual change in the curvature on each cross-section. If the support at B was released so that a vertical displacement at B was possible, the member ABC would gradually deﬂect upwards at B due to the creep-induced hogging curvature associated with the primary moment Pe on each cross-section. If it is assumed that the creep characteristics are uniform and the prestressing force is constant throughout, the time-dependent curvature caused by creep on each crosssection can be determined using the procedure presented in Section 5.4. For lightly reinforced cross-sections, the creep-induced curvature (κk )cr may be taken as a product of the instantaneous curvature and the creep coefﬁcient (Eq. 8.11a) and the upward displacement at B is given by Eq. 8.11b: (κk )cr = uB (τk ) =

Pe ϕ(τk , τ0 ) Ec I

(8.11a)

(κk )cr L2 2

(8.11b)

where I is the second moment of area of the transformed section about its centroidal axis. In Eq. 8.11a, it is assumed that the restraint offered to creep by the bonded reinforcement is insigniﬁcant. If the amount of bonded reinforcement is signiﬁcant, a more accurate approximation may be made by dividing the creep coefﬁcient in Eqs 8.11 by the parameter α deﬁned in Section 3.6.6 and, for uncracked cross-sections, speciﬁed in Eq. 3.32b.

322 Members and structures The deﬂection at B caused by a unit value of the vertical redundant reaction force gradually applied at the release at B may be calculated using the procedures of Section 8.3.2. An approximation for the time-dependent ﬂexibility coefﬁcient associated with the release at B is given by: L3 [1 + χ (τk , τ0 )ϕ(τk , τ0 )] L3 = f¯11 = 6Ec I 6 Ee I

(8.12)

The redundant force at B that gradually develops with time RB (τk ) is obtained from Eq. 8.6: RB (τk ) = −

uB (τk ) 3Pe ϕ(τk , τ0 ) ≈− ¯f11 L 1 + χ(τk , τ0 )ϕ(τk , τ0 )

= RB

ϕ(τk , τ0 ) 1 + χ(τk , τ0 )ϕ(τk , τ0 )

(8.13)

where RB is the hyperstatic reaction that would have developed at B if the structure was initially continuous and later prestressed with a straight tendon of constant eccentricity e. In general, if R is any hyperstatic reaction or the restrained internal action that would occur at a point due to prestress in a continuous member and R(t) is the corresponding creep-induced value if the member is made continuous after the application of prestress, then: RB (t) ≈

ϕ(τk , τ0 ) R 1 + χ(τk , τ0 )ϕ(τk , τ0 )

(8.14)

If the creep characteristics of the concrete are uniform throughout the structure, then Eq. 8.14 may be applied to systems with any number of redundants. Providing continuity at the interior supports of a series of simple precast beams, not only restrains the time-dependent deformation caused by prestress, but also restrains the deformation caused by external loads. For all the external loads applied after the continuity is established, the effects can be calculated by moment distribution or an equivalent method of structural analysis. Under the loads applied to the simplysupported beams prior to casting the joints (such as the self-weight of the precast beams), the moments at each interior support are initially zero. However, after the joint has been cast, the creep-induced deformations resulting from these selfweight moments are restrained and moments develop with time at the supports. For the two-span beam shown in Fig. 8.20, the initial moment at the support B due to self-weight is zero. However, if the beam had initially been continuous over the interior support, the moment at B would have been MB = wsw L2 /8. The moment that develops with time due to creep at support B due to creep and self-weight is: MB (t) ≈

ϕ(τk , τ0 ) MB 1 + χ(τk , τ0 )ϕ(τk , τ0 )

Members and structures

323

Example 8.6 Consider two simply-supported pretensioned concrete planks, erected over two adjacent spans as shown in Fig. 8.20. An in-situ reinforced concrete joint is cast at the interior support, to provide continuity. Each plank is 1000 mm wide by 150 mm thick and pretensioned with straight strands at a constant depth of 110 mm below the top ﬁbre, with Ap = 400 mm and Pp,init = 500 kN. A typical cross-section is shown in Fig. 8.21. The span of each plank is L = 6 m. If it is assumed that the continuity is provided immediately after the transfer of prestress, the reactions that develop with time due to creep are to be determined. For convenience, and to better illustrate the effects of creep in this situation, shrinkage is not considered and the self-weight of the planks is also ignored. The material properties are: Ec = 30,000 MPa; fct = 3.0 MPa; ϕ(τk , τ0 ) = 2.0; χ (τk , τ0 ) = 0.65; εsh = 0; and Ee = 13,040 MPa. 1000 150 110

Ap = 400 mm2 Pp,init = 500 kN

Figure 8.21 Cross-section of planks in Example 8.6 (all dimensions in mm).

Immediately after transfer, and before any creep has taken place, the curvature on each cross-section caused by the eccentric prestress may be calculated using the procedure outlined in Section 5.3 giving κ0 = −2.02 × 10−6 mm−1 . The top and bottom ﬁbre concrete stresses are σtop,0 = 1.30 MPa and σtop,0 = −7.81 MPa, so that cracking has not occurred. In the absence of any restraint at the supports, the curvature on each crosssection would change with time due to creep from κ0 to κk = −5.81×10−6 mm−1 (calculated using the procedure outlined in Section 5.4). If the support at B in Fig. 8.20 was removed, the deﬂection at B (uB (τk )) that would occur with time due to the change in curvature caused by creep ((κk )cr = κk −κ 0 = −3.79 × 10−6 mm−1 ) can be calculated from Eq. 8.1b for the 12 m long planks and is also given by Eq. 8.11b: uB (τk ) =

−3.79 × 10−6 × 60002 = −68.2 mm (i.e. upward) 2

The deﬂection at B caused by a unit value of the vertical redundant reaction force gradually applied at the release at B is calculated using the procedures of Section 8.3.2 and for this example is given by Eq. 8.12. With the second moment of area of the age-adjusted transformed cross-section I = 288.3 × 106 mm4 , Eq. 8.12 gives: L3 60003 f¯11 = = = 9.58 × 10−3 6 Ee I¯ 6 × 13,040 × 288.3 × 106

324 Members and structures and the redundant force at B that gradually develops with time, RB (τk ) is therefore: RB (τk ) = −

uB (τk ) −68.2 =− = 7124 N ¯f11 0.00958

The reaction that would have developed at B due to prestress immediately after transfer if the member had initially been continuous is RB = 8621 kN and the approximation of Eq. 8.14 gives: RB (τB ) ≈

2.0 × 8621 = 7497 N 1 + 0.65 × 2.0

In this example, Eq. 8.14 gives a value for RB (τk ) that is within 6 per cent of the value determined above and provides a quick and reasonable estimate of the effects of creep. The secondary moment at B that develops with time due to prestress is 21.4 kNm and this is 83 per cent of the secondary moment that would have developed if the two planks had been continuous at transfer.

8.4 Two-way slab systems 8.4.1 Discussion The design of suspended concrete slab systems is complicated by the difﬁculties involved in estimating the service load behaviour. It is relatively easy to ﬁnd a load path and reinforce a slab to satisfy the requirements of adequate strength. Slabs are usually very ductile, highly indeterminate members that are capable of considerable moment redistribution as the ultimate load is approached. The distribution of moments in a statically indeterminate slab at failure is very much dependent on the reinforcement pattern and, therefore, on the load path assumed in design. However, in the design for serviceability, the distribution of moments and the prediction of deﬂection at service loads are far more uncertain. The distribution of moments varies with time and depends on the extent of cracking, the post-cracking stiffness of the various parts of the slab, the level of creep and shrinkage and the restraint provided at the supports. As outlined in the preceding pages, the initial and time-dependent deformations and the extent of cracking in concrete structures depend primarily on the non-linear and inelastic properties of concrete and, as such, are difﬁcult to predict with conﬁdence. The problem is exacerbated in the case of slabs which are typically thin in relation to their spans and are therefore more deﬂection sensitive. It is stiffness rather than strength that controls the design of most reinforced and prestressed concrete slab systems. The ﬁrst step in the design of a two-way slab panel is the initial selection of the slab thickness. A reasonable ﬁrst estimate is desirable since, in many cases, the slab selfweight is a large portion of the total service load. The initial estimate is often based on personal experience or on recommended maximum span-to-depth ratios or minimum thickness requirements, such as those presented in Section 3.5. While providing a useful starting point in design, such a selection does not necessarily ensure serviceability. Deﬂections at all critical stages in the history of the slab must be calculated and

Members and structures

325

the magnitudes limited to acceptable design values. Failure to adequately predict deﬂections has frequently resulted in serviceability problems (Ref. 4). The procedures discussed so far in this chapter have been concerned with the prediction of the in-service behaviour of line members, such as beams, one-way slabs and frames. For the calculation of two-way slab deﬂections, several additional problems need to be overcome. The three-dimensional nature of the slab, the less well deﬁned inﬂuence of cracking and tension stiffening and the development of biaxial creep and shrinkage strains must all be modelled adequately. In addition, the ﬁnal deﬂection of a slab depends very much on the extent of initial cracking which, in turn, depends on the construction procedure (the shoring and reshoring sequence), the amount of early shrinkage, the temperature gradients in the ﬁrst few weeks after casting, the degree of curing and so on. Many of these parameters are, to a large extent, outside the control of the designer. In ﬁeld measurements of the deﬂection of many identical slab panels (Refs 5 and 6), a large variability was reported. Deﬂections of identical panels after one year differed by over 100 per cent in some cases. These differences can be attributed to the different conditions that existed in the ﬁrst few weeks after casting of each slab, including differences in both the applied load and the environmental conditions. In more recent laboratory tests on large-scale ﬂat slabs, a change in deﬂection at least as large as that caused by the full design live load was observed after exposing the top surface of a dry slab to rainwater (Ref. 7). Nevertheless, various approximate methods are available that may be used to predict ball-park estimates of the deﬂection of two-way slabs, making use of the cross-sectional analyses presented in Chapters 4–7. By varying the amount of early cracking, for example by varying the tensile strength of concrete, upper and lower bounds on deﬂection can be obtained. Some approximate procedures for deﬂection calculation are reviewed in the following sections. 8.4.2 Slab deﬂection models In view of the complexities and uncertainties involved in estimating the service load behaviour of two-way slab systems, great accuracy in the calculation of deﬂection is neither possible nor warranted. Nevertheless, numerous approximate techniques are available for the prediction of moments and deformations in concrete slab systems. These range from relatively simple procedures to sophisticated research models. The small deﬂection theory of elastic plates can be used to predict slab deﬂections. Deﬂection coefﬁcients for elastic slabs with ideal boundary conditions and subjected to full panel loading have been presented by Timoshenko and Woinowsky-Krieger (Ref. 8). Many more simple models involve the analysis of orthogonal slab strips. The deﬂection of the slab panel is approximated by the sum of the deﬂection components of one or more slab strips (see Refs 9–15). The ﬁnite-element method is perhaps the most powerful and potentially the most accurate tool for the analysis of concrete slabs. The basic method is well established and has been described in many text books. Since the early 1970s, many investigators have developed non-linear ﬁnite-element models to study the short-term service load behaviour of reinforced concrete slabs. A number of researchers extended their models to handle the time-dependent effects of creep and shrinkage (e.g. Refs 16–18). Today numerous commercial ﬁnite element software packages are available to undertake non-linear analysis of slabs at service loads. The treatment of time effects in these

326 Members and structures computer packages ranges from rational and reliable to crude and unreliable. Users of any commercial program should be aware of the assumptions made in the modelling of material non-linearity, particularly relating to cracking, creep and shrinkage, and make a rational assessment of the reliability of the output. However, ﬁnite element modelling of two-way slab systems, even with the most reliable of software, is time consuming and generally unsuitable for routine use in structural design. However, it is a useful research tool to examine the effects of various parameters on slab behaviour and to generate the parametric data necessary for the development of more simple, design-oriented procedures for the estimation of slab deﬂections. Such parametric studies have been reported elsewhere (Ref. 17) and have led to the development of simple, design-oriented methods for the deﬂection control of slabs (Ref. 15). The ﬁnite-element model described in Ref. 17 has been used for the calibration of slab stiffness factors in the following section. 8.4.3 Two-way edge-supported slabs This section deals with the prediction of the deﬂection of two-way rectangular slab panels that are continuously supported on all four edges by beams or walls and that carry a uniformly distributed load. The slab panel may be either continuous or discontinuous on each edge. A simple and useful estimate of deﬂection may be made using the so-called crossing beam analogy. This involves the consideration of a pair of orthogonal slab strips of unit width spanning through the centre of the panel as shown in Fig. 8.22. Each slab strip carries only part of the transverse load w on the slab. By equating the mid-span deﬂection of each slab strip and assuming that the entire transverse load is carried by bending in the two orthogonal directions, the fraction of load carried in the short-span direction γ ∗ is easily determined. If each strip is initially assumed to be uncracked: γ∗ =

L4y λL4x + L4y

(8.15)

where λ depends on the support conditions of the panel and is given by: λ = 1.0 λ = 1.0 λ = 2.0 λ = 0.5 λ = 2.5 λ = 0.4 λ = 5.0 λ = 0.2

for 4 edges continuous discontinuous for 2 adjacent edges discontinuous for 1 long edge discontinuous for 1 short edge discontinuous for 2 long + 1 short edge discontinuous for 2 short + 1 long edge discontinuous for 2 long edges discontinuous for 2 short edges discontinuous.

The deﬂection of the slab may be estimated conservatively by calculating the initial and time-dependent deﬂection of the shorter span slab strip subjected to a uniformly distributed load, γ ∗ w. However, this ignores the torsional stiffness of the slab and violates compatibility at all but the slab centre. As a consequence, the predicted deﬂection may be signiﬁcantly greater than the actual deﬂection. Using the non-linear

Members and structures

327

Lx = short span Ly = long span

1m

Equivalent slab strip

Panel is continuously supported along all edges

Figure 8.22 Orthogonal slab strips in an edge-supported slab.

ﬁnite-element model described in Ref. 17, a slab stiffness factor has been calibrated which may be used to adjust the stiffness of the shorter span beam, so that the deﬂection of the slab panel is predicted more accurately. In Table 8.4, this slab stiffness factor is combined with the value of γ ∗ (as given by Eq. 8.15). The deﬂection of the panel may be estimated by analysing a unit wide one-way slab strip in the short span direction with the same boundary conditions as the relevant slab edges and carrying uniformly distributed load of γ ∗ w. For each possible boundary condition, γ ∗ depends on the aspect ratio Ly /Lx and may be interpolated from Table 8.4. If the slab edges are supported by beams, the average deﬂection of the supporting beams along the long edges must be calculated and added to the slab strip deﬂection to obtain the total deﬂection at the centre of the panel. Table 8.4 Values of γ ∗ for two-way edge-supported slabs Value of γ ∗ Ly /Lx

4 edges continuous 1 short edge discontinuous 1 long edge discontinuous 2 short edges discontinuous 2 long edges discontinuous 2 adjacent edges discontinuous 2 short + 1 long edge discontinuous 2 long + 1 short edge discontinuous 4 edges discontinuous

1.0

1.25

1.5

2.0

5.0

0.48 0.60 0.31 0.74 0.15 0.45 0.55 0.22 0.36

0.70 0.78 0.50 0.87 0.28 0.66 0.71 0.36 0.50

0.84 0.91 0.69 0.95 0.41 0.79 0.81 0.50 0.60

0.94 0.97 0.87 0.99 0.65 0.93 0.94 0.72 0.80

1.00 1.00 1.00 1.00 0.97 1.00 1.00 1.00 1.00

Example 8.7 The maximum ﬁnal deﬂection at the mid-span of a 6 by 8 m exterior panel of a beam and slab ﬂoor system is to be calculated. The slab panel is 150 mm thick and forms part of the ﬂoor of a retail store. The panel edges are continuously supported by stiff beams. The design moments in the slab have been

328 Members and structures determined from moment coefﬁcients speciﬁed in the local building code and the reinforcement has been calculated to satisfy the design objective of adequate strength. Top and bottom reinforcement plans are shown in Fig. 8.23, together with the relevant material properties. All reinforcement bars are Australian Class N (normal ductility) 12 mm diameter deformed bars spaced at centres shown in millimetres. Bars in the short-span direction are placed closest to the bottom of the slab and closest to the top, as shown, with the effective depth d = 150 − 20 − 6 = 124 mm. 8m

8m

A

D

D

A th

st

N12@300 (4 )

N12@180 (1 )

6m

rd

N12@170 (3 )

nd

N12@230 (2 )

B

th

N12@130 (4 )

C

Stiff beams

N12@170 (3rd)

(a) Bottom reinforcement plan

B

C

(b) Top reinforcement plan

f c′ = 25 MPa ; Ec = 25,000 MPa ; f* = 2.8 ; c* = 0.8 ; e*sh =

−0.0006 ; fy = 500 MPa ; Es = 200,000 MPa ; ft = 2.0 MPa ; Minimum concrete cover = 20 mm

Figure 8.23 Details of 150 mm thick slab panel of Example 8.7.

The slab carries a superimposed dead load of gsup = 1.5 kPa, in addition to its own self-weight gsw , and the speciﬁed live load q is 5.0 kPa. For a retail store, the service load factors are taken as (refer to Section 3.3) ψ1 = 0.6 (for short-term loads) and ψ2 = 0.3 (for long-term loads). If reinforced concrete is taken to weigh 24 kN/m3 , then the sustained load is: wsus = gsw + gsup + ψ2 q = 24 × 0.15 + 1.5 + 0.3 × 5.0 = 6.6 kPa and the variable load is: wvar = (ψ1 − ψ2 )q = (0.6 − 0.3) × 5.0 = 1.5 kPa The slab panel is discontinuous on one long edge only, with an aspect ratio of Ly /Lx = 1.33, and from Table 8.4 γ ∗ = 0.56. A 1 m wide slab strip spanning in the short-span direction through the slab centre is to be analysed. The slab strip is considered to be continuous at one end and simply-supported at the other, as shown in Fig. 8.24a. The analysis of such a member was presented in Example 8.4. Assume the bending moment produced by the maximum short-term load on the strip (i.e. γ ∗ (wsus + wvar ) = 4.54 kN/m) is as shown in Fig. 8.24b.

Members and structures MBC = −20.0 kNm/m

N12@300 = 367 mm2/m

N12@130 = 846 mm2/m

g *w = 4.54 kN/m 150 mm

B-C 6m

N12@180 = 611 mm2/m A-D

329

A-D

B-C Mmid-span = 10.43 kNm/m Mmax = 11.65 kNm/m

(a) Elevation

(b) Bending moment diagram

Figure 8.24 Elevation of slab strip and moment diagram in Example 8.7.

From a short-term cross-sectional analysis using the approach outlined in Section 5.3, the cracking moments for this 150 mm thick slab at mid-span at ﬁrst loading (with zero shrinkage) and at the interior support are +9.89 and −10.09 kNm/m. It is evident that both the positive and negative moment regions of the slab will crack under the full service load. The initial and time-dependent curvatures at each support and at mid-span caused by the sustained load γ ∗ wsus = 3.70 kN/m and the short-term curvatures caused by the variable load γ ∗ wvar = 0.84 kN/m are calculated using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked sections and Sections 7.2 and 7.3 for the cracked sections and are summarised in Table 8.5. From the uncracked analyses, the moments required to produce an extreme ﬁbre tensile stress in the concrete of fct = 2.5 MPa at ﬁrst loading τ0 and at τk are readily determined and given in Table 8.5. Tension stiffening is accounted for using the distribution factor ζ given in Eq. 8.3 and the average curvature κavge at each critical section due to each loading is calculated using Eq. 8.2 and is also given in Table 8.5. Table 8.5 Uncracked, cracked and average curvature at critical sections in Example 8.7. At continuous support

At mid-span

At discontinuous support

At ﬁrst loading, τ0

Final at τk

At ﬁrst loading, τ0

Final at τk

At ﬁrst Final at loading, τ0 τk

Cracking moment, Mcr (kNm/m)

−10.09

−4.64

9.89

5.99

–

–

Max. moment, Ms∗ (kNm/m)

−20.0

−20.0

11.65

11.65

0

0

Distribution factor, 0.746 ζ (Eq. 8.3)

0.946

0.279

0.736

0

0

Due to γ ∗ wvar : κuncr (mm−1 )

−0.50 × 10−6

−0.50 × 10−6

0.27 × 10−6

0.27 × 10−6 0

0

(mm−1 )

−2.18 × 10−6

−2.18 × 10−6

1.48 ×

10−6

1.48 × 10−6 0

0

κavge (mm−1 )

−1.75 × 10−6

−2.09 × 10−6

0.61 × 10−6

1.16 × 10−6 0

0

Due to γ ∗ wsus + shrinkage: κuncr (mm−1 ) κcr (mm−1 )

−2.21 × 10−6 −9.60 × 10−6

−9.20 × 10−6 −20.0 × 10−6

1.17 × 10−6 5.33 × 10−6

6.52 × 10−6 0 14.8 × 10−6 0

0.77 × 10−6 –

κavge (mm−1 )

−7.42 × 10−6

−19.4 × 10−6

2.33 × 10−6

12.6 ×−6

0.77 × 10−6

κcr

0

330 Members and structures The short-term deﬂection at mid-span due to the variable loading at time τk is obtained from Eq. 8.1b: (vc )var =

60002 (−2.09 + 10 × 1.16 + 0) × 10−6 = 3.6 mm 96

and the long-term deﬂection due to the sustained load and shrinkage is (vc )sus =

60002 (−19.4 + 10 × 12.6 − 0.77) × 10−6 = 39.6 mm 96

The maximum total panel deﬂection is therefore (vc )max = (vc )var + (vc )= sus 43.2 mm. With a maximum deﬂection of span/130, this slab is unserviceable for most applications and a thicker slab would almost certainly be required for this ﬂoor system.

8.4.4 Flat slabs In this section, a simple method is presented for predicting the deﬂection at the midpanel of a uniformly loaded two-way column-supported ﬂat slab. The basic procedure is known as the wide beam method (or equivalent frame method) and was formalised by Nilson and Walters (Ref. 19). It is assumed here that the design bending moments in each direction are known and that the quantity and layout of the reinforcement in each region of the slab are also known: that is, the slab has been designed for strength and an estimate of deﬂection is now required. The basis of the method is illustrated in Fig. 8.25. For the deﬂection calculation, the deformation of a slab panel in one direction at a time is considered. The contributions in each direction are then added to obtain the total deﬂection. In Fig. 8.25a, the slab is considered to act as a wide, shallow beam of width equal to the panel dimension Ly and span equal to Lx and carrying the entire load in the x-direction. This wide beam is assumed to rest on unyielding supports. Because of variations in moment and ﬂexural rigidity across the width of the slab, all unit strips in the x-direction will not deform identically. Moments, and hence curvatures, in the regions near the column lines (the column strip) are greater than in the middle strips. The deﬂection on the column line is therefore greater than that at the panel centre. This is particularly so, when, as is usually the case, the column strips are cracked and the middle strips are uncracked. The slab is next considered to act as a wide shallow beam carrying the entire load in the y-direction as shown in Fig 8.25b. Once again, the effect of variation of moment and ﬂexural rigidity across the panel is shown. The mid-panel deﬂection is taken to be the sum of the average mid-span deﬂection of the column strips in one direction (usually taken as the long-span direction) and the mid-span deﬂection of the middle strip in the other direction (Fig. 8.25c). That is:

vcx1 + vcx2 vmax = + vmy (8.16) 2

Members and structures

331

y

Assumed support line

vcx2 vmx

vcx1 Lx

Ly

y Assumed support line

x

(a) x–direction bending

vmy vcy2 Lx

Ly

y x vmax

(b) y–direction bending

Lx

Ly (c) Two-way bending x

Figure 8.25 Deﬂection components of a ﬂat slab (Ref. 19).

The method is fully compatible with the equivalent frame method of moment analysis (Ref. 20). The deﬁnition of column and middle strips, the longitudinal moment distribution, lateral moment distribution coefﬁcients and other details are the same as for the moment analysis, so that in design most of the information required for the estimation of deﬂection has been previously calculated. With the moment diagrams for the column and middle strips known, it is a simple matter to determine the curvatures at the supports and at the mid-span of each strip, using the cross-sectional analyses of Chapters 5 and 7. The initial and time-dependent strip deﬂections can be calculated using Eq. 8.1b. For ﬂat slabs, the span in Eq. 8.1b may be taken to be the centre to centre distance between columns or the clear span (face to face of columns) plus the slab depth, whichever is smaller.

Example 8.8 The maximum total deﬂection at the mid-point of a square interior panel of the ﬂat plate shown in Fig. 8.26 is to be calculated. The slab is 200 mm thick and supports a sustained service load of wsus = 6.3 kPa (which includes self-weight) and a variable live load of wvar = 3.0 kPa. The column and middle strips in each direction are 3575 mm wide. The tensile reinforcement quantities in the x-direction column strip and y-direction middle strip are given in Table 8.6. The steel in the x-direction is placed ﬁrst and

332 Members and structures f c′

Column strip

= 25 MPa; Ec = 25,000 MPa;

fct = 3.0 MPa; fy = 500 MPa; f* =

2.5;

c* =

0.65;

e*sh =

Middle strip

7.15 m 6.75 m

−0.0006

y

D = 200 mm

x

Column strip

Effective span, Le = Ln + D = 6.95 mm

6.75 m 7.15 m

Figure 8.26 Slab details and material properties for Example 8.8.

last (i.e. closest to the top and bottom surfaces of the slab) and the steel in the y-direction is placed in the second and third layers. If 20 mm cover and 16 mm diameter bars are assumed, the effective depths in each direction are: dx = 200 − 20 − 8 = 172 mm dy = dx − 16 = 156 mm Also shown in Table 8.6 are the peak positive and negative in-service bending moments caused by wsus +wvar in each strip. These were calculated in accordance with the direct design method of slab design (see Ref. 20). Table 8.6 Steel quantities and in-service moments for Example 8.8 Column strip (x-direction)

Middle strip (y-direction)

Negative Positive Negative moment region moment region moment region Ast (mm2 ) 5420 Msus+var (kNm) −196

2280 85

1950 −66

Positive moment region 1650 56

Column strip deﬂection (x-direction) At the support The maximum in-service moment in the column strip at the support (due to wsus + wvar ) is −196 kNm and, from the cross-section analysis of Section 5.3, the cracking moment at ﬁrst loading is −80.0 kNm and after all shrinkage is −32.8 kNm. The critical cross-section at the support will obviously be cracked. The ﬁnal time-dependent curvature at the support caused by the moment due to the sustained load (Msus = −132.8 kNm) plus shrinkage and the short-term curvature caused by the moment due to the variable load (Mvar = −63.2 kNm) are calculated using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked section and Sections 7.2 and 7.3 for the cracked section and are

Members and structures

333

summarised below. For the inclusion of tension stiffening in the ﬁnal deﬂection calculations, the distribution factor ζ at time τk is obtained from Eq. 8.3: ζ = 1−

−32.8 −196

2 = 0.972

and the average curvatures at the supports of the column strip are obtained from Eq. 8.2. Instantaneous curvature due to Mvar : κuncr = −0.98×10−6 mm−1 ;κcr = −3.19×10−6 mm−1 ; and therefore κavge = −3.13×10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = −7.85×10−6 mm−1 ;κcr = −14.23×10−6 mm−1 ; and therefore κavge = −14.05×10−6 mm−1 . At mid-span The maximum in-service moment in the column strip at mid-span (due to wsus + wvar ) is 85 kNm and, from Section 5.3, the cracking moment at ﬁrst loading is 75.1 kNm and after all shrinkage is 56.0 kNm. The critical cross-section at mid-span will crack. The ﬁnal time-dependent curvature at mid-span caused by the moment due to the sustained load (Msus = 57.6 kNm) plus shrinkage and the short-term curvature caused by the moment due to the variable load (Mvar = 27.4 kNm) are next determined using the cross-sectional analyses of Sections 5.3 and 5.4 for the uncracked section and Sections 7.2 and 7.3 for the cracked section. The distribution factor ζ at time τk is obtained from Eq. 8.3:

56.0 ζ = 1− 85

2 = 0.566

and the average curvatures at mid-span of the column strip are obtained from Eq. 8.2: Instantaneous curvature due to Mvar : κuncr = 0.44×10−6 mm−1 ;κcr = 2.79×10−6 mm−1 ; and therefore κavge = 1.77 ×10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = 3.81×10−6 mm−1 ;κcr = 11.71×10−6 mm−1 ; and therefore κavge = 8.28×10−6 mm−1 .

334 Members and structures Deﬂection The short-term deﬂection at mid-span of the column strip due to the variable loading is: 69502 (−3.13 + 10 × 1.77 + −3.13) × 10−6 = 5.8 mm 96

(vcx )var =

and the long-term deﬂection due to the sustained load and shrinkage is: 69502 (−14.05 + 10 × 8.28 − 14.05) × 10−6 = 27.5 mm 96

(vcx )sus =

The maximum total panel deﬂection at mid-span of the columns strip is therefore: (vcx )max = (vcx )var + (vcx )sus = 33.3 mm

Middle strip deﬂection (y-direction) The cracking moment for the middle strip at the support after all shrinkage has taken place is −58.4 kNm and at mid-span is 60.4 kNm, so the strip may suffer minor cracking at the support line (where from Table 8.6 the maximum in-service moment Msus+var = −66 kNm) but will be uncracked at mid-span (where Msus+var = 56 kNm). At the support At time τk : ζ = 1−

−58.4 −66

2 = 0.217

Due to Mvar : κuncr = −0.35 × 10−6 mm−1 ; κcr = −3.05 × 10−6 mm−1 ; and therefore κavge = −0.94 × 10−6 mm−1 Final long-term curvature due to Msus + shrinkage: κuncr = −3.01 × 10−6 mm−1 ; κcr = −12.77 × 10−6 mm−1 ; and therefore κavge = −5.13 × 10−6 mm−1 . At mid-span Due to Mvar : κavge = κuncr = 0.30 × 10−6 mm−1 Due to Msus + shrinkage: κavge = κuncr = 2.58 × 10−6 mm−1 . Deﬂection The short-term deﬂection at mid-span of the middle strip due to the variable loading is: (vmy )var =

69502 (−0.94 + 10 × 0.30 − 0.94) × 10−6 = 0.6 mm 96

Members and structures

335

and the long-term deﬂection due to the sustained load and shrinkage is:

(vmy )sus =

69502 (−5.13 + 10 × 2.58 − 5.13) × 10−6 = 7.8 mm 96

The maximum total panel deﬂection at mid-span of the middle strip in the ydirection is: (vmy )max = (vmy )var + (vmy )sus = 8.4 mm

Panel deﬂection Finally, the maximum deﬂection at the mid-point of the panel is obtained from Eq. 8.16: vmax =

33.3 + 33.3 + 8.4 = 41.7 mm 2

8.5 Slender reinforced concrete columns 8.5.1 Discussion In most structural members, creep and shrinkage of concrete cause increases of deformation and redistribution of stresses, but do not affect strength. In some situations, however, the deformations caused by creep and shrinkage can lead to an increase in the loads on the structure and, therefore, a reduction in strength. A slender column under sustained, eccentric compression is such an example. Other examples include shallow concrete arches and domes. Consider the slender pin-ended column shown in Fig. 8.27. The column is subjected to a compressive force P applied at an initial eccentricity e0 . When P is ﬁrst applied at time τ0 , the column shortens and deﬂects laterally by an amount δ0 . The bending moment at each end of the column is Pe0 , but at the column mid-length, the moment is P(e0 + δ0 ). Therefore, the lateral deﬂection of the member causes an increase in the internal actions. For long columns, the secondary moment Pδ0 may be many times greater than the initial primary moment Pe0 and the load-carrying capacity is much less than that of a short column with the same cross-section. For very long columns, an instability failure may occur under relatively small compressive loads, i.e. buckling may occur before the strength of the cross-section at mid-length is reached. For reinforced concrete columns under sustained loads, the member suffers additional lateral deﬂection due to creep. This time-dependent deformation leads to additional bending in the member, which in turn causes the column to deﬂect still further. During a period of sustained loading, an additional deﬂection δ(t) will develop at the mid-length of the column. The gradual increase in the secondary moment with time P(δ0 + δ(t)) reduces the factor of safety and, for long columns, creep buckling may occur.

336 Members and structures P

P A

C

e0

(a) Initial geometry

P e0 A

e0

C

d0

C

P (b) At time t0

PDd(t) P d0 P e0

e0 d0 + Dd(t)

B

B P

P A

B P (c) At time t

P e0 (d) Bending moments

Figure 8.27 Displacements and moments in a slender pin-ended column.

In order to design slender reinforced concrete columns for the strength limit state, an accurate assessment of the creep deformation is necessary to ensure an adequate factor of safety. In the following section, an iterative computer-based procedure for the analysis of slender reinforced concrete columns is presented. 8.5.2 An iterative method of analysis To account for the geometric non-linearity associated with the secondary actions in a slender column (Pδ0 + Pδ(t)), as well as the material non-linearity associated with cracking, creep and shrinkage, an iterative solution procedure that uses the AEMM to include the time effects is described here. The analyses of cross-sections in the uncracked parts of the column are undertaken using the method described in Sections 5.3 and 6.2 (for short-term analysis) and Sections 5.4 and 6.3 (for long-term analysis), while for cross-sections in the cracked parts of the column, the analyses are undertaken in accordance with Section 7.2 (for short-term behaviour) and Section 7.3 (for time-dependent behaviour). Consider again the pin-ended column shown in Fig. 8.27. The iterative solution procedure involves the following steps: (i) The member is subjected initially to the axial load P and the primary moment Pe0 on every cross-section. The initial strain distributions and curvatures are calculated at the cross-sections at each end of the member (i.e. at A and B) and at the midlength (C). (ii) The lateral deﬂection of the member at the mid-length of the column, δ0 , is determined from the initial curvatures calculated in step (i). If a parabolic variation of curvature along the member is assumed, δ0 may be calculated using Eq. 8.1b. (iii) The additional increment of moment caused by δ0 at the mid-length of the columns (Pδ0 ) is added to the primary moment and the cross-section at C is re-analysed. The curvature at C is now larger than that calculated in step (i), and so too is the

Members and structures

337

lateral deﬂection δ1 at the mid-length of the column (re-calculated using Eq. 8.1b). The revised secondary moment (Pδ1 ) is added to the primary moment at C and the cross-section is again reanalysed. The procedure continues until the lateral displacement at C converges to δi after the ith iteration. The short-term response of the slender column is thus determined. The lateral deﬂection at C immediately after loading (δi ) is known, as is the stress and strain distributions on the cross-sections at A, B and C. If the member is very slender, convergence may not occur in step (iii) and a buckling instability may result. The secondary moment Pδ calculated during the iterative cycle, may cause cracking on a previously uncracked cross-section and therefore result in considerable loss of stiffness and an increase in the lateral displacement and secondary moment. The number of iterations required for convergence therefore depends on the slenderness of the member, the initial eccentricity and the tensile strength of the concrete. In step (iii), convergence may be deemed to occur when the additional lateral displacement calculated at mid-length during the ith iteration (δi – δi−1 ) is less than 0.001 of the lateral displacement δ0 caused by the primary moments and calculated in step (ii). With the behaviour immediately after loading at τ0 determined in step (iii), the time analysis commences: (iv) The time-dependent changes in strain and curvature at A, B and C are calculated using the previously speciﬁed time analyses. Initially, the internal actions at C (P and P(e0 + δi )) are assumed to remain constant with time. The change in the lateral displacement at C (δ0 ) caused by the change in curvature with time at each cross-section is calculated using Eq. 8.1b. This increase in displacement with time causes an additional increment of secondary moment Pδ0 to be applied gradually to the cross-section at C. This time-dependent secondary moment, in turn, produces additional lateral displacements and additional increments of secondary moment. An iterative procedure is again followed until the time-dependent lateral displacement converges to δ(t) (or until instability occurs). To model behaviour using the AEMM, the time-dependent increments of secondary moment, which in fact occur gradually, are applied to the age-adjusted transformed cross-section at mid-span. For initially cracked cross-sections, the depth to the neutral axis is assumed to remain constant with time. As was discussed in Section 7.3, this assumption, although not correct, is a reasonable compromise between accuracy and economy of solution. A more reﬁned analysis could be implemented to trace the development of time-dependent cracking using the SSM based on the iterative procedure outlined in Section 7.4.

Example 8.9 A pin-ended column with the cross-section shown in Fig. 8.28 is subjected to a constant sustained axial compressive load P = 500 kN acting at a constant eccentricity of e0 = 65 mm. The behaviour of the column is to be determined,

338 Members and structures both at ﬁrst loading τ0 and at time inﬁnity, for each of the following three column lengths: (i) L = 6000 mm; (ii) L = 7500 mm; and L = 9000 mm. Material properties are: Ec = 25,000 MPa; Es = 200,000 MPa; fc = 25 MPa; ft = 2.5 MPa; φ ∗ (τ0 ) = 2.5; fct = 2.5 MPa; φ ∗ (τ0 ) = 2.5; χ ∗ (τ0 ) = 0.65; and ∗ = 0. εsh 300

60

As = 900 mm2

P = 500 kN x

As = 900 mm2

180

65

60 y

Figure 8.28 Column section for Example 8.9 (all dimensions in mm).

Case (i): L = 6000 mm The initial stresses and strains on each cross-section due to the axial force P = 500 kN and the moment Pe0 = 32.5 kNm are calculated using the crosssectional analysis described in Section 5.3. In this case, the primary moment and axial force at each end and at mid-length are the same. On each cross-section, the compressive strain at the reference x-axis and curvature are εr,0 = −195 × 10−6 and κ0 = 1.673 × 10−6 mm−1 and the extreme ﬁbre concrete stresses are σtop = −11.15 MPa and σbot = +1.40 MPa. Since the tensile strength of the concrete is not exceeded, the member is uncracked. The lateral displacement at the column mid-length caused by the primary moment is obtained from Eq. 8.1b: δo =

60002 (1.673 + 10 × 1.673 + 1.673) = 7.53 mm 96

and the increment of secondary moment at the column mid-length Pδ0 = 3.76 kNm. This secondary moment is added to the primary moment and the cross-section at mid-length is re-analysed. The revised curvature at midlength is (κi )1 = 1.841 × 10−6 mm−1 and the revised displacement at mid-length is calculated using Eq. 8.1b is δ1 = 8.16 mm. The corresponding secondary moment is Pδ1 = 4.08 kNm. The revised secondary moment is added to the primary moment and the section at C is again re-analysed. The procedure continues for two more iterations until the lateral deﬂection converges to δi = 8.33 mm. The stress and strain distributions at mid-length are εr,0 = −195 × 10−6 ; κ0 = 1.887 × 10−6 mm−1 ; σtop = −11.95 MPa; and σbot = +2.20 MPa. The section at mid-length therefore remains uncracked.

Members and structures

339

For the time analysis, the cross-sections at each end and at the mid-length of the column are analysed using the procedure outlined in Section 5.4. Initially, the internal actions are assumed to remain constant. The change in the lateral displacement at mid-length caused by the change in curvature on each crosssection with time is δ0 = 14.23 mm. The secondary moment Pδ0 is applied to the age-adjusted transformed cross-section at mid-length, thus producing an additional increment of displacement and secondary moment. Convergence occurs after ﬁve iterations. The time-dependent change in displacement at the column mid-length is δi = 17.73 mm. The column therefore suffers a total mid-length lateral deﬂection of δi + δi = 26.06 mm. The initial and ﬁnal strain distributions and concrete stresses on the crosssections at each end and at the mid-length of the column are illustrated in Fig. 8.29. It is noted that the ﬁnal bottom ﬁbre tensile stress exceeds the tensile stress of the concrete indicating that cracking in the mid-length region of the column is likely to occur with time. −1216

−11.15 −7.86

−446

Initial Final

56 144 Strain (× 10−6)

0.9 1.4 Concrete stress (MPa)

(a) At each end of the column −1368

−478

−11.95 −9.62

Initial Final

88 428 Strain (× 10−6)

2.2 2.98 Concrete stress (MPa)

(b) At the mid-length of the column

Figure 8.29 Stresses and strains for case (i) of Example 8.9.

Case (ii): L = 7500 mm The stress and strain distributions at each end of the column are the same as those calculated in case (i). However, the increased column length results in larger lateral displacements and increased secondary moments. The secondary moments in this case are large enough to cause cracking at the mid-length of the column at initial loading. The initial and ﬁnal lateral displacements at the column mid-length in case (ii) are δi = 16.43 mm and δi + δ = 69.71 mm and the corresponding strains and stresses on the cross-section at mid-length are shown in Fig. 8.30a.

340 Members and structures

Case (iii): L = 9000 mm In this case, the initial column deﬂection at mid-length is δi = 30.03 mm and the initial states of stress and strain on the cross-section at the mid-point of the column are shown in Fig. 8.30b. As time progresses, additional secondary moments caused by creep become so large that convergence does not occur and the member buckles. For such a slender member, creep deformations result in a reduction of strength with time. −2043

−543

−14.68 −13.56 219.7

Initial Final 3.19 198 Strain (× 10−6)

1265 Concrete stress (MPa) (a) Case (ii)

−628

−15.69 Initial 194.6

Creep buckling occurs with time! 0

340 Strain (× 10−6)

Concrete stress (MPa)

(b) Case (iii)

Figure 8.30 Stresses and strains at the column mid-length for Example 8.9.

8.6 Temperature effects 8.6.1 Introduction A uniform or linearly varying temperature distribution through the depth of a statically determinate homogeneous member causes the member to deform, but no stress is produced on any cross-section. In practice, however, temperature rarely varies linearly through the depth of a member and members are usually unable to accommodate the deformation caused by temperature change without some restraining forces developing at the supports. Because plane sections tend to remain plane, a non-linear temperature gradient produces internal, self-equilibrating eigenstresses, as illustrated in Fig. 8.31. The free expansion (or contraction) of each concrete ﬁbre is restrained by the adjacent ﬁbres resulting in the internal stress distribution shown. A similar distribution of selfequilibrating internal stress is produced by non-linear shrinkage and was discussed in Section 1.3.3 and illustrated in Fig. 1.13. Usually design engineers are concerned with temperature changes applied over a short time period. If the temperature gradient is sustained for a period of time, the

Members and structures

341

To Elastic + creep strain

s(y)

Unrestrained temperature strain = αT(y)

T(y)

Total strain

(a) Temperature change

(b) Strain

(c) Self-equilibrating stress

Figure 8.31 Effects of non-linear temperature distribution on cross-sectional response.

internal stresses induced by temperature are relieved, to some extent, by creep. If necessary, a time analysis using the AEMM can be used to determine the variation of cross-sectional behaviour with time. In a statically indeterminate member, the displacement at the member’s ends caused by the axial deformation and curvature induced by temperature may not be free to occur. Reactions develop at the supports and internal actions are induced at each cross-section of the member. The stresses resulting from these secondary actions can be large and must be calculated and added to the stresses illustrated in Fig. 8.31, if the total stresses on a cross-section of a statically indeterminate member are required. The determination of these continuity stresses is discussed in Section 8.6.4. 8.6.2 Temperature distributions Temperature variations caused by solar radiation in bridge decks, for example, can produce stress levels that are of similar magnitude to those produced by the gravity loads, even if the structure is statically determinate. In the design of such structures, an analysis to determine the effects of temperature often plays an important part. Design codes provide guidance on temperature gradients that should be considered for particular structural applications. For example, typical temperature proﬁles to be used in the design of composite concrete-concrete bridges are shown in Fig. 8.32 and are based on the Australian speciﬁcations (Refs 21 and 22). 8.6.3 Temperature analysis of cross-sections In this section, the short-term analysis of a cross-section subjected to an arbitrary nonlinear temperature variation at time τ0 is presented. The overall method of analysis is similar to that presented in Sections 5.3–5.7, except that a thermal-induced strain is included in the constitutive relationship of each constituent material. For a reinforced or prestressed concrete cross-section with mc concrete components, ms layers of non-prestressed reinforcement and mp layers of prestressing tendons, the constitutive relationships are: σc(i),0 = Ec(i),0 ε0 − εc(i),T

(8.17a)

342 Members and structures Max Dd = 300 mm y

Ttop

0.4Ttop

24°C

300

300 300

D

Ttop +3 T(°C) Dd

6°C

T(y) = Ttop + 3 − 0.05y Temperature profile across deck slabs over closed box cells (shaded area)

D

T(y) = Ttop 1− 200

(a) Concrete deck on girder (Ref. 21)

y 5 1200

5 if soffit is within 8 m of ground 0 if over water y (mm)

(b) Box girder bridge deck (Ref. 22)

Figure 8.32 Temperature gradients for concrete box girders (Refs 21–22).

σs(i),0 = Es(i) ε0 − εs(i),T σp(i),0 = Ep(i) ε0 + εp(i),init − εp(i),T

(8.17b) (8.17c)

where εc(i),T , εs(i),T and εp(i),T are the thermal-induced strains in the concrete, nonprestressed reinforcement and prestressing tendons, respectively, and are determined from: εc(i),T = αc(i),T T (y)

(8.18a)

εs(i),T = αs(i),T T (y)

(8.18b)

εp(i),T = αp(i),T T (y)

(8.18c)

in which T(y) is the temperature distribution on the cross-section as a function of distance y from the reference axis, and αc(i),T , αs(i),T and αp(i),T are the coefﬁcients of thermal expansion for the concrete, non-prestressed reinforcement and prestressing tendons, respectively. The contributions to the internal axial force on the cross-section of the constituent materials at time τ0 after the temperature change are: Nc,0 =

mc

σc(i),0 dA =

i=1A c(i)

−

mc i=1A c(i)

mc

Ac(i) Ec(i),0 εr,0 +

i=1

Ec(i),0 εc(i),T dA

mc

Bc(i) Ec(i),0 κ0

i=1

(8.19a)

Members and structures Ns,0 =

ms

As(i) Es(i) εr,0 +

i=1

ms

ys(i) As(i) Es(i) κ0 −

i=1

ms

As(i) Es(i) εs(i),T

343

(8.19b)

i=1

mp mp mp Np,0 = Ap(i) Ep(i) εr,0 + yp(i) Ap(i) Ep(i) κ0 + Ap(j) Ep(i) εp(i),init i=1

i=1

i=1

mp

−

Ap(i) Ep(i) εp(i),T

(8.19c)

i=1

Combining these contributions, the internal axial force and bending moment resisted by the whole cross-section are: mp Ni,0 = Nc,0 +Ns,0 +Np,0 = RA,0 εr,0 +RB,0 κ0 + Ap(j) Ep(j) εp(j),init −NT,0 j=1

(8.20a) mp

Mi,0 = Mc,0 +Ms,0 +Mp,0 = RB,0 εr,0 +RI,0 κ0 +

yp(i) Ap(i) Ep(i) εp(i),init −MT,0 i=1

(8.20b) where the cross-sectional rigidities at time τ0 , i.e. RA,0 , RB,0 and RI,0 , have already been deﬁned in Eqs 5.72, and NT,0 and MT,0 are the equivalent actions required to produce the same deformation as the temperature change if each material was unrestrained and are given by: NT,0 =

mc

Ec(i),0 εc(i),T dA +

i=1A c(i)

mp ms As(i) Es(i) εs(i),T + Ap(i) Ep(i) εp(i),T i=1

i=1

(8.21a) MT,0 =

mc

yEc(i),0 εc(i),T dA +

i=1A c(i)

ms ys(i) As(i) Es(i) εs(i),T i=1

mp yp(i) Ap(i) Ep(i) εp(i),T +

(8.21b)

i=1

Substituting Ni,0 and Mi,0 (Eqs 8.20) into Eqs 5.2, the equilibrium equations may be expressed as: re,0 = D0 ε0 + fp,init − fT

(8.22)

and solving Eq. 8.22 gives the unknown strain variables ε0 : ε0 = D−1 re,0 − fp,init + fT = F0 re,0 − fp,init + fT 0

(8.23)

344 Members and structures where ε0 , re,0 , D0 , F0 and f p,init are all deﬁned in Eqs 5.71 and f T is given by:

NT,0 fT = MT,0

(8.24)

Evaluation of the integral expressing the thermal response of the concrete can be carried out numerically or in closed form when the temperature variation is speciﬁed with a known function.

Example 8.10 The stress and strain distributions on the section shown in Fig. 8.33a caused by the temperature gradient shown in Fig. 8.33b are to be calculated. The cross-section is of a statically determinate beam and the rise in temperature is applied over a short time period. Because temperature rises are associated with expansion, they are here taken to be positive. The coefﬁcient of thermal expansion for both concrete and steel is αc = αs = 10 × 10−6 /o C and the prestressing steel is bonded to the surrounding concrete. Take Ec = 30,000 MPa and Es = Ep = 200,000 MPa. 400 200

20°C 100

200

200

As2 = 400 mm2 200

x

600 2

Ap = 2000 mm

y

2°C

300

As2 = 1240 mm2 200 100

200

(a) Cross-section

20

300 0

T(y)

5°C

eT = αT(y)

50

(b) Temperature gradient

(c) Free temperature induced strain

Figure 8.33 Section details and temperature gradient for Example 8.9.

The free temperature strain εT = αT(y) is shown in Fig. 8.33c and the equivalent actions NT,0 in each material are: NTc,0 =

mc

Ec(i),0 εc(i),T dA = [400 × 200 ×

i=1A c(i)

+ 200 × 300 ×

(200 − 20) + 400 × 200 × 20 2

50 20 + 400 × 200 × − 400 × 110 2 2

− 1240 × 25] × 10−6 × 30,000 = 339.8 kN

Members and structures NTs,0 =

345

ms As(i) Es(i) εs(i),T = [400 × 110 + 1240 × 25] × 10−6 × 200,000 i=1

= 15.0 kN mp NTp,0 = Ap(i) Ep(i) εp(i),T = [2000 × 200,000 × 0] = 0 i=1

and the moments of these forces about the centroidal axis of the section are: MTc,0 =

mc

yEc(i),0 εc(i),T dA = [400 × 200 ×

i=1A c(i)

(200 − 20) ˙ × (−433.3) 2

+ 400 × 200 × 20 × (−400) + 200 × 300 × + 400 × 200 ×

20 × (−200) 2

50 × 433.3 − 400 × 110 × (−400) 2

− 1240 × 25 × 400] × 10−6 × 30,000 = −90.25 kNm MTs,0 =

ms ys(i) As(i) Es(i) εs(i),T = [400 × 110 × (−400) i=1

+ 1240 × 25 × 400] × 10−6 × 200,000 = −1.04 kNm mp yp(i) Ap(i) Ep(i) εp(i),T = [300 × 2000 × 200,000 × 0] = 0 NTp,0 = i=1

From Eqs 8.21: NT,0 = NTc,0 + NTs,0 + NTp,0 = 354.8 kN MT,0 = MTc,0 + MTs,0 + MTp,0 = −90.25 − 1.04 = −91.29 kNm The rigidities of this cross-section are obtained from Eqs 5.72 as RA,0 = 9.02 × 109 N, RB,0 = 15.91 × 1010 Nmm, RI,0 = 9.67 × 104 Nmm2 , and with the F0 matrix for this cross-section calculated using Eq. 5.71b, the strain matrix for the otherwise unloaded cross-section is determined using Eq. 8.23:

−1.829 × 10−14 1.112 × 10−10 ε0 = F0 fT = −14 −1.829 × 10 1.037 × 10−15 41.1 × 10−6 = −0.1012 × 10−6 mm−1

354.8 × 103 −91.29 × 106

346 Members and structures The top (y = −500 mm) and bottom (y = +500 mm) ﬁbre strains are: ε0,top = 41.1 × 10−6 + (−500) × (−0.1012 × 10−6 ) = 91.7 × 10−6 ε0,bot = 41.1 × 10−6 + 500 × (−0.1012 × 10−6 ) = −9.5 × 10−6 The temperature-induced changes of stress in the concrete are determined from Eq. 8.17a as follows: At y = −500 mm: σ c,0 = 30,000[41.1 + (−500) × (−0.1012) − 200] × 10−6 = −3.25 MPa At y = −300 mm: σc,0 = 30,000[41.1 + (−300) × (−0.1012) − 20] × 10−6 = 1.54 MPa At y = 0 mm: σc,0 = 30,000[41.1 + (0) × (−0.1012) − 0] × 10−6 = 1.23 MPa At y = +300 mm: σc,0 = 30,000[41.4 + (300) × (−0.1012) − 0] × 10−6 = 0.32 MPa At y = +500 mm: σc,0 = 30,000[41.4 + (500) × (−0.1012) − 50] × 10−6 = −1.79 MPa From Eqs 8.17b and c: σs(1) = 200,000[41.4 + (−400) × (−0.1012) − 110] × 10−6 = −5.68 MPa σs(2) = 200,000[41.4 + (400) × (−0.1012) − 25] × 10−6 = −4.88 MPa σp = 200,000[41.4 + (300) × (−0.1012) − 0] × 10−6 = −2.15 MPa The temperature-induced strains and eigenstresses on the concrete section are shown in Fig. 8.34. 91.7

200

−3.25

−

20

1.54

Free temperature strain, eT +

1.23

Actual strain, e0

0.32 − −9.5

50

Strain (×10−6)

−1.79

Concrete stress (MPa)

Figure 8.34 Temperature-induced stress and strain in Example 8.10.

Members and structures

347

8.6.4 Temperature effects in members and structures The temperature-induced strains on individual cross-sections cause axial deformation and rotation of members and structures. In statically indeterminate members, the displacement caused by temperature changes may not be free to occur, and restraining forces may develop at the supports. The stresses and deformations caused by these restraining forces must be calculated and added to the temperature-induced eigenstresses in order to obtain the total effect of temperature. The redundant forces caused by restraint to temperature can be determined using exactly the same procedure as outlined in Section 8.3.2.

Example 8.11 A beam with cross-section shown in Fig. 8.33a is subjected to the temperature gradient of Fig. 8.33b applied over its entire length in an eight-hour period. If the beam was statically determinate, the temperature-induced stresses and strains on the cross-section were calculated in Example 8.10 and illustrated in Fig. 8.34. From Example 8.10, the temperature-induced strain at the reference axis (at the mid-depth of the cross-section) and the curvature on each cross-section of the beam are: εr,0 = 41.1 × 10−6 and κ0 = −0.1012 × 10−6 mm−1 .

(a) The beam is uncracked throughout and simply supported over a span of 14 m The displacement of the beam (idealised in Fig. 8.35a) is to be determined. The axial deformation of the member is: eAB = εr,0 L = 41.1 × 10−6 × 14,000 = 0.58 mm (elongation) and the deﬂection at mid-span is calculated using Eq. 8.1b: vC =

14,0002 12 × (−0.1012) × 10−6 = −2.48 mm 96 θA

A

vC

C L = 14,000 mm

eAB B

(a) Simply-supported beam MA

VA

VB (b) Redundant reactions if end A is fixed

Figure 8.35 Temperature-induced deformations and reactions in Example 8.11.

348 Members and structures From Eq. 3.7b, the slope at each end of the beam is: θA = θB =

14,000 3 × (−0.1012 × 10−6 ) = −0.708 × 10−3 rad 6

(b) The support at A is ﬁxed, so that θA is prevented If the rotation at A cannot occur, the temperature gradient will induce the reactions shown in Fig. 8.35b at the supports. For this analysis, the moment at A is taken to be the redundant, RR = MA , and the deformation of the primary structure at the release is: uA = θA = −0.708 × 10−3 Due to a unit moment applied at A, the rotation at A is f11 and the reactions at the supports of the primary beam are RPR , where: L f11 = 3Ec I

and RPR =

2 ! VA = −1 L 2 VB = +1 L

For this beam, Ec = 30,000 MPa and the second moment of are of the transformed cross-section about its centroidal axis is equal to I = 31,040 ×106 mm4 . Therefore: ¯f11 =

14,000 = 5.01 × 10−12 3 × 30,000 × 31,040 × 10−6

From Eq. 8.5, the redundant moment at A is:

RR = MA = −

−0.708 × 10−3 = 141.3 kNm 5.01 × 10−12

and the other reactions of the statically indeterminate beam are determined from statics: VB =

MA 141.3 × 106 = = 10.09 kN L 14,000

and VA = −VB = −10.09 kN

The temperature-induced eigenstresses at the support A were calculated in Example 8.10 and are reproduced in Fig. 8.36a. In Fig. 8.36b, the continuity stresses in the concrete caused by the redundant moment MA are also shown. The resultant temperature-induced stresses are obtained by summing the eigenstresses and the continuity stresses and are illustrated in Fig. 8.36c.

Members and structures −3.25

−5.55

−2.30

−

− 0.16

−

1.54 + 1.23

349

+

1.22

= +

0.32 − −1.79 (a) Eigenstresses

1.66

+ +2.25 (b) Continuity stresses

0.46 (c) Resultant stresses

Figure 8.36 Temperature-induced concrete stresses at ﬁxed support at A in Example 8.11.

8.7 Concluding remarks The techniques described and illustrated in this chapter may be extended readily to include a wide range of additional structural applications. The procedures are not daunting and require little more than an elementary background in mechanics and structural analysis. An analysis for the effects of creep and shrinkage on the behaviour of concrete structures allows the structural design engineer to better predict and control inservice performance. But perhaps of greater importance, it provides a clear picture of the interaction between concrete and reinforcement at service loads and a better understanding of why concrete structures behave as they do.

8.8 References 1. British Standards Institution (2004). Eurocode 2: Design of Concrete Structures – part 1-1: General rules and rules for buildings BS EN 1992-1-1: 2004. European Committee for Standardization, Brussels. 2. Ghali, A. and Neville, A.M. (1978). Structural Analysis – A Uniﬁed Classical and Matrix Approach. Chapman and Hall, London. 3. Hall, A.S. and Kabaila, A.P. (1977). Basic Concepts of Structural Analysis. Pitman Publishing, London. 4. Mayer, H. and Rüsch, H. (1967). Building Damage Caused by Deﬂection of Reinforced Concrete Building Components. Technical Translation 1412, National Research Council Ottawa, Canada (Deutscher Auschuss für Stahlbeton, Heft 193, Berlin, West Germany). 5. Sbarounis, J.A. (1984). Multi-storey ﬂat plat buildings – measured and computed one-year deﬂections. Concrete International, 6(8), 31–35. 6. Jokinen, E.P. and Scanlon, A. (1985). Field measured two-way slab deﬂections. CSCE Annual Conference, Saskatoon, Canada, May. 7. Gilbert, R.I. and Guo, X.H. (2005). Time-dependent deﬂection and deformation of reinforced concrete ﬂat slabs – an experimental study. ACI Structural Journal, 102(3), 363–373.

350 Members and structures 8. Timoshenko, S. and Woinowsky-Krieger, S. (1959). Theory of Plates and Shells. McGrawHill Book Co., New York. 9. Marsh, C.F. (1904). Reinforced Concrete. D. Van Nostrand Co., New York. 10. Ewell, W.W., Okuba, S. and Abrams, J.I. (1952). Deﬂections in gridworks and slabs. Transactions, ASCE, 117, p. 869. 11. Furr, W.L. (1959). Numerical method for approximate analysis of building slabs. ACI Journal, 31(6), 511. 12. Vanderbilt, M.D., Sozen, M.A. and Siess, C.P (1963). Deﬂections of Reinforced Concrete Floor Slabs. Structural Research Series No. 263, Department of Civil Engineering, University of Illinois, April. 13. Rangan, B.V. (1976). Prediction of long-term deﬂections of ﬂat plates and slabs. ACI Journal, 73(4), 223–226. 14. Nilson. A.H. and Walters, D.B. (1975). Deﬂection of two-way ﬂoor systems by the equivalent frame method. ACI Journal, 72(5), 210–218. 15. Gilbert, R.I. (1985). Deﬂection control of slabs using allowable span to depth ratios. ACI Journal, 82(1), 67–72. 16. Scanlon, A. and Murray, D.W. (1974). Time-dependent reinforced concrete slab deﬂections. Journal of the Structural Division, ASCE, 100, 1911–1924. 17. Gilbert, R.I. (1979). Time-Dependent Behaviour of Structural Concrete Slabs. PhD Thesis, University of New South Wales, pp 361. 18. Chong, K.T., Foster, S.J. and Gilbert, R.I. (2008). Time-dependent modelling of RC structures using the cracked membrane model and solidiﬁcation theory. Computers and Structures, 86(11–12), 1305–1317. 19. Nilson, A.H. and Walters, D.B. (1975). Deﬂection of two-way ﬂoor systems by the equivalent frame method. ACI Journal, 72(5), 210–218. 20. American Concrete Institute (2008). Building Code Requirements for Reinforced Concrete ACI 318M-08 and Commentary. ACI Committee 318, Michigan, USA. 21. National Association of State Road Authorities (1992). NAASRA – Bridge design speciﬁcation. Sydney. 22. Standards Australia (2004). Bridge Design Part 2: Design Loads AS5100.2-2004. Sydney.

9

Stiffness method and ﬁnite-element modelling

9.1 Introduction The analysis of members and frames is commonly carried out in design ofﬁces using commercial software based on either the stiffness method or the ﬁnite-element approach. This chapter outlines how these methods can be used for the long-term analyses of concrete structures, accounting for the effects of creep and shrinkage. The solution procedures required for the methods are well established (Refs 1–3) and only a brief overview of them is provided here. Throughout the chapter frequent reference is made to Appendix A, where the detailed derivations required to establish the proposed approaches are outlined. Worked examples are also presented to better illustrate the methods.

9.2 Overview of the stiffness method The stiffness method of analysis, also referred to as the displacement method, is a matrix method for the analysis of complex structural systems using computers. A beam or frame is discretised into a number of line elements, referred to as stiffness elements, connected at their ends by nodes. A typical two-dimensional six degree of freedom (6 DOF) frame element of length L is illustrated in Fig. 9.1, where the three possible displacement components at each end node and the three corresponding nodal actions are shown. The overall structural response is evaluated by combining the contribution of each single element in resisting the applied loads or deformations. This approach relies on the fact that, for each element, it is possible to establish a stiffness relationship between nodal actions and nodal displacements, i.e.: p = ke u

(9.1)

where p and u are the nodal actions and displacements of an element, and ke is the element stiffness matrix. For any particular element, this relationship is expressed in its particular coordinate system (usually referred to as the local or member

352 Stiffness method and ﬁnite-element modelling coordinate system). For example, for the 6 DOF frame element of Fig. 9.1, the stiffness matrix is derived in Appendix A as Eq. A.51 and is reproduced here as: ⎡

RA ⎢ ⎢ L ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ RB ⎢− ⎢ L ke = ⎢ ⎢ ⎢ RA ⎢− ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎣ R B L

0 12 α1 L 3 6 α1 L 2 0 −

12 α1 L3

6 α1 L 2

RB − L 6 α1 L2 R2 4 + B α 1 L RA L

RA − L

RB L 6 − α1 L2 R2 2 − B α 1 L RA L

RA L

0

0

12 α 1 L3

0

0

−

12 α1 L 3

RB L

−

6 α1 L 2

−

RB L

−

6 α1 L 2

⎤ RB ⎥ ⎥ L ⎥ ⎥ 6 ⎥ ⎥ α1 L2 ⎥ ⎥ R2B ⎥ 2 ⎥ − α1 L R A L ⎥ ⎥ ⎥ ⎥ RB ⎥ − ⎥ L ⎥ ⎥ 6 ⎥ − ⎥ α1 L 2 ⎥ ⎥ R2B ⎦ 4 + α1 L R A L

(9.2a)

and the nodal actions and displacements shown in Fig. 9.1 are: ⎡

⎤ NL ⎢ ⎥ ⎢ SL ⎥ ⎢ ⎥ ⎢ ML ⎥ ⎢ ⎥ p=⎢ ⎥ ⎢ NR ⎥ ⎢ ⎥ ⎣ SR ⎦ MR ⎡ ⎤ uL ⎢ ⎥ ⎢ vL ⎥ ⎢ ⎥ ⎢ θL ⎥ ⎥ u=⎢ ⎢u ⎥ ⎢ R⎥ ⎢ ⎥ ⎣ vR ⎦ θR

(9.2b)

(9.2c)

The rigidities RA , RB and RI have been introduced in Chapters 5 and 7 for different types of cross-sections, and the coefﬁcients α0 and α1 are calculated from the rigidities using Eqs A.50a and b. The subscripts ‘L’ and ‘R’ on the nodal loads and displacements denote the left (at z = 0) and right (at z = L) member ends, respectively, when looking at the element with the z-axis horizontal and pointing towards the right. In the proposed formulation, the coordinate system is illustrated in Fig. 9.2 for a typical reinforced concrete member. To remain consistent with the coordinate systems adopted in previous chapters, rotations are assumed to be positive when clockwise and transverse displacements are positive when in the direction of the y-axis. In a real structure, members may have different orientations (with different local coordinate systems). It is therefore convenient to introduce a global coordinate system to be used for the whole structure. The load and displacement vectors for a particular

Stiffness method and ﬁnite-element modelling 353 qR

MR

uR

SR

vR uL

NL

L z

vL

qL

NR

ML

L SL

z

(b) Nodal actions

(a) Nodal displacements

Figure 9.1 Freedoms of the 6 DOF frame element.

z

L x y

Figure 9.2 Coordinate system adopted for the member analysis.

element (deﬁned in local coordinates in Eqs 9.2b and c, respectively) can be expressed in global coordinates by carrying out the following transformations: u = TUe

(9.3a)

Pe = TT p

(9.3b)

where Pe represents the load vector in global coordinates, Ue is the vector of nodal displacements in global coordinates, and the transformation matrix T is given by: ⎡

c s 0 0 0 ⎢ ⎢−s c 0 0 0 ⎢ ⎢ ⎢0 0 1 0 0 T=⎢ ⎢0 0 0 c s ⎢ ⎢ ⎣ 0 0 0 −s c 0 0 0 0 0

⎤ 0 ⎥ 0⎥ ⎥ ⎥ 0⎥ ⎥ 0⎥ ⎥ ⎥ 0⎦ 1

(9.4)

where c and s are, respectively, the cosine and the sine of the angle between the global and local coordinate systems (measured clockwise from the global system).

354 Stiffness method and ﬁnite-element modelling Substituting Eqs 9.3 into Eq. 9.1 gives the stiffness relationship of a particular element expressed in global coordinates: Pe = Ke Ue

(9.5)

where Ke is the stiffness matrix of the element in global coordinates given by: K e = T T ke T

(9.6)

The stiffness relationship for the whole structure is then obtained by assembling the contribution of each element and can be expressed as: P = KU

(9.7)

where K is the structural stiffness matrix, while P and U are, respectively, the vectors of nodal actions and displacements for the whole structure expressed in the global coordinate system. Equation 9.7 is readily solved for the unknown displacements and reactions. For illustrative purposes, Eq. 9.7 can be re-written in terms of the known and unknown displacements (UK and UU ) and known and unknown actions (PK and PU ) as follows: K11 K12 UU PK = (9.8) PU K21 K22 UK The unknown displacements and actions are determined as follows: −1 UU = K11 (PK − K12 UK )

(9.9a)

PU = K21 UU + K22 UK

(9.9b)

9.3 Member loads Distributed member loads can be considered in the analysis by introducing particular sets of nodal actions that produce equivalent effects to the original distributed loads and, for this reason, are usually referred to as equivalent nodal loads. These correspond to the opposite of the reactions that would occur at the end of a loaded stiffness element if its ends were assumed to be ﬁxed. Different sets of equivalent nodal loads have been derived in Appendix A. For example, in the case of uniform longitudinal and transverse distributed loads (referred to as n and p, respectively, in Fig. 9.3), the end reactions of a ﬁxed ended member pF.m are given in Eq. A.52 (reproduced here for ease of reference): ⎡ ⎤ ⎡ ⎤ 0 −L/2 ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ α3 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢Lα3 /2⎥ (9.10) pF.m = ⎢ ⎥ p+⎢ ⎥n ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ −L/2 ⎦ ⎣ α3 ⎦ L2 /12 Lα3 /2

Stiffness method and ﬁnite-element modelling 355 p NL ML

NR SL

n

SR

MR

Figure 9.3 Free body diagram of a frame element highlighting uniformly distributed vertical and horizontal member loads n and p.

The subscript ‘m’ indicates that the reactions relate to member loads, while the subscript ‘F’ indicates that these actions have been determined assuming both ends of the element are fully ﬁxed. The term α3 is the ratio of the cross-sectional rigidities RB and RA and is deﬁned in Eq. A.50d. The equivalent nodal loads for inclusion in the stiffness analysis are the opposite of these reactions (i.e. −pF.m ). The unknown displacements and reactions of the structure are obtained from Eqs 9.9 after the nodal loads from all elements are assembled. The actions on each element (depicted in Fig. 9.1b) can be calculated by adding the forces and moments caused by the calculated displacements (= ku) to the ﬁxed-end reactions speciﬁed in Eq. 9.10 as: p = ku + pF.m

(9.11)

Based on the Euler–Bernoulli beam assumptions, the displacements at any point along the length of an element are given by: z4 z3 z2 4 + C1 + C 2 + C 3 z + C 24 6 2 z2 z3 6 5 z + C +C u = α2 p + α3 C 1 + α4 n 6 2 v = α1 p

(9.12a) (9.12b)

where these equations are derived in Appendix A as Eqs A.53. The terms α1 , α2 , α3 and α4 are calculated from the cross-sectional rigidities and are given in Eqs A.50b–e. 1 to C 6 are obtained by specifying the appropriate The constants of integration C boundary conditions and are expressed in terms of the nodal (element) displacements and applied member loads in Eqs A.54. The expressions describing the variation of the axial strain (measured at the level of the x-axis) and curvature along the member length can be obtained by differentiating Eqs 9.12: u = α2 p

z2 5 + α3 C1 + α4 n z + C 2

(9.13a)

v = α1 p

z2 2 + C1 z + C 2

(9.13b)

356 Stiffness method and ﬁnite-element modelling For example, these expressions can be used to evaluate the internal axial force and moment resisted by the concrete (Eqs A.56 and A.58) which will become useful in the following sections dealing with time effects: Nc = Ac Ec u − Bc Ec v = ac0 + ac1 z + ac2 z2

(9.14a)

Mc = Bc Ec u − Ic Ec v = bc0 + bc1 z + bc2 z2

(9.14b)

The concrete cross-sectional properties have been deﬁned in Chapter 5, while the use of the parabolic polynomial to describe the variation of both Nc and Mc is justiﬁed in Appendix A for the derivation of Eqs A.56 and A.58. The coefﬁcients of the polynomials (ac0 , ac1 , ac2 , bc0 , bc1 , bc2 ) are given in Appendix A (Eqs A.57 and A.59). In the following example, a simple beam subdivided into two elements is considered for illustrative purposes only. Clearly, the method is more applicable for more complex structures.

Example 9.1 The instantaneous mid-span deﬂection of the simply-supported beam shown in Fig. 9.4 is to be determined using the stiffness method. The beam is subjected to the uniformly distributed transverse load and the axial point load shown. The set of external actions reproduces the loading condition of Example 5.1 at midspan of the member. The analysis is carried out using two stiffness elements of equal length numbered 1 and 2, respectively, as shown in Fig. 9.4. The geometry and material properties of the cross-section are as speciﬁed in Example 5.1 (including the use of the x-axis located at 200 mm below the top ﬁbre of the cross-section). The member actions for both elements are to be calculated, as are all the coefﬁcients necessary to deﬁne the expressions for the strain and for the internal actions resisted by the concrete along each element. 4 kN/m 30 kN 1

B

2

A 5m

5m

C

Figure 9.4 Loading, support conditions and discretisation for Example 9.1.

All units utilised in the solutions are in mm and N. For clarity, units are not displayed next to the terms in large matrices in the following solution. An additional subscript ‘(1)’ or ‘(2)’ is used to specify whether a variable is calculated for elements 1 or 2, respectively. Where variables are identical for both elements, the subscript might be omitted for ease of notation. This is usually the case for the cross-sectional rigidities and material properties that are identical for both elements. The freedoms for the problem are numbered in Fig. 9.5, where the lower numbers are used for the unrestrained freedoms. This numbering strategy is particularly useful for hand calculation as it leads to the partitioning introduced

Stiffness method and ﬁnite-element modelling 357 in Eqs 9.8. Also for this particular example, with the numbering proposed in Fig. 9.5, global and local coordinates coincide and there is no need to include transformations between the two coordinate systems in the solution, such as those described in Eqs 9.3 and 9.6.

1

A 8

7 1

2

B 3

2 4

C 9

5 6

Figure 9.5 Freedom numbering for Example 9.1.

Considering that freedoms 7, 8 and 9 are restrained by the pinned and roller supports, their displacements are known, while the displacements along the remaining freedoms are unknown. Therefore: T T T UK = U7 U8 U9 = 0 0 0 and UU = U1 U2 U3 U4 U5 U6 The unknown reactions are collected in PU : PU = P7

P8

P9

T

From Example 5.1, the instantaneous cross-section rigidities are: RA = 4923 × 106 N RB = 543.9 × 109 Nmm RI = 221.0 × 1012 Nmm2 and from Eqs A.50: α0 = R1 RA − R2B = 792.3 × 1021 N2 mm2 α1 =

RA = 6.214 × 10−15 N−1 mm−2 α0

α2 =

RB = 686.5 × 10−15 N−1 mm−1 α0

α3 =

RB = 110.5 mm RA

α4 = −

1 = −203.1 × 10−12 N−1 RA

358 Stiffness method and ﬁnite-element modelling The stiffness matrices for elements 1 and 2 are identical (as both possess the same geometric and cross-sectional properties) and are given by Eq. 9.2a: ⎡ ⎤ 984.7 × 103 0 −108.8 × 106 −984.7 × 103 0 108.8 × 106 ⎢ ⎥ ⎢ ⎥ ⎢ 15.45 × 103 38.62 × 106 0 −15.45 × 103 38.62 × 106 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ 9 6 6 9 140.7 × 10 108.8 × 10 −38.62 × 10 52.35 × 10 ⎥ ⎢ ⎥ k=⎢ ⎥ ⎥ ⎢ 3 6 ⎢ 984.7 × 10 0 −108.8 × 10 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ sym 15.45 × 103 −38.62 × 106 ⎥ ⎣ ⎦ 140.7 × 109

The ﬁxed end forces on each element due to the transverse load p = 4 N/mm are obtained from Eq. 9.10: ⎤ 0 ⎥ ⎢ ⎢ L⎥ ⎢− ⎥ ⎢ 2 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ L2 ⎥ ⎢− ⎥ ⎢ 12 ⎥ ⎥ pF.m(1) = pF.m(2) = ⎢ ⎥ ⎢ ⎢ 0 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ L⎥ ⎢− ⎥ ⎢ 2 ⎥ ⎥ ⎢ ⎣ L2 ⎦ 12

⎡

⎡

⎤

⎢ ⎥ 0N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢−8.3 × 106 Nmm⎥ ⎢ ⎥ p=⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎣ ⎦ 8.3 × 106 Nmm

Assembling the contribution of the two elements into the stiffness matrix of the structure enables the determination of the various sub-matrices of K given in Eq. 9.8: ⎡ ⎤ 140.7 × 109 108.8 × 106 −38.62 × 106 52.35 × 109 0 0 ⎢ ⎥ ⎢ ⎥ ⎢ 1.969 × 106 0 −217.6 × 106 −984.7 × 103 108.8 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 30.89 × 103 0 0 38.62 × 106 ⎥ ⎢ ⎥ K11 = ⎢ ⎥ 9 6 9 ⎥ ⎢ 281.5 × 10 108.8 × 10 52.35 × 10 ⎢ ⎥ ⎢ ⎥ 3 6⎥ ⎢ sym 984.7 × 10 −108.8 × 10 ⎣ ⎦

⎡

−108.8 × 106 ⎢ ⎢−984.7 × 103 ⎢ ⎢ 0 ⎢ K12 = ⎢ ⎢ 108.8 × 106 ⎢ ⎢ 0 ⎣ 0

38.62 × 106 0 −15.45 × 103 38.62 × 106 0 0

0

⎤

⎥ ⎥ ⎥ ⎥ −15.45 × 103 ⎥ ⎥ −38.62 × 106 ⎥ ⎥ ⎥ 0 ⎦ 6 −38.62 × 10 0

140.7 × 109

⎡ ⎢ K22 = ⎣

984.7 × 103

Stiffness method and ﬁnite-element modelling 359 ⎤ 0 0 ⎥ ⎦ 15.45 × 103 0 15.45 × 103

sym T K21 = K12

Assembling the load vector for the whole structure (including the axial load of −30 kN applied at freedom 5) produces: ⎡

⎤ 8.3 × 106 Nmm ⎢ ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢ 20 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 0 Nmm ⎢ ⎥ ⎢ 3 P = ⎢ −30 × 10 N ⎥ ⎥ ⎢ ⎥ ⎢−8.3 × 106 Nmm⎥ ⎢ ⎥ ⎢ ⎥ P7 ⎢ ⎥ ⎢ ⎥ 3 ⎣ P8 + 10 × 10 N ⎦ P9 + 10 × 103 N Unknown displacements UU and reactions PU are then calculated using Eqs 9.9: ⎡

1.138 × 10−3

⎤

⎢ ⎥ ⎢−156.2 × 10−3 mm⎥ ⎢ ⎥ ⎢ ⎥ 3.494 mm ⎢ ⎥ −1 UU = K11 (PK − K12 UK ) = ⎢ ⎥ ⎢ ⎥ 0 ⎢ ⎥ ⎢ ⎥ −3 ⎣−312.5 × 10 mm⎦ −1.138 × 10−3 ⎤ ⎡ ⎤ 30 × 106 N P7 ⎢ ⎥ ⎢ ⎥ PU = ⎣P8 ⎦ = ⎣−20 × 106 N⎦ P9 −20 × 106 N ⎡

The mid-span deﬂection is the displacement related to freedom 3) and is equal to 3.49 mm.

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element.

360 Stiffness method and ﬁnite-element modelling Element 1 The nodal displacements undergone by the end nodes of element 1 are collected in vector u(1) : ⎤

⎡

⎡ ⎤ u 0 mm L(1) ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢v ⎥ 0 mm ⎢ L(1) ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ v ⎥ ⎢ −3 ⎢ ⎥ 1.138 × 10 ⎥ ⎢ ⎥ u(1) = ⎢ L(1) ⎥ = ⎢ ⎢ ⎥ ⎥ ⎢ −3 mm⎥ ⎢uR(1) ⎥ ⎢ −156.2 × 10 ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢vR(1) ⎥ ⎣ 3.494 mm ⎦ ⎦ ⎣ vR(1)

0

The member actions are obtained from Eq. 9.11: p(1) = ku(1) + pF.m(1) T = 30 × 103 N −20 × 103 N 0 Nmm −30 × 103 N 0 N −50 × 106 Nmm The relevant constants of integration are then obtained from Eqs A.54: 1(1) = −124.3 × 10−12 mm−2 C 2(1) = −20.59 × 10−9 mm−1 C 3(1) = 1.138 × 10−3 C 4(1) = 0 mm C 5(1) = −8.368 × 10−6 C 6(1) = 0 mm C These can be substituted in Eqs 9.13 to determine the strain distribution along member 1. For example, the axial strain measured at the level of the ) at mid-span of the reference axis εr(1) (= u(1) ) and the curvature κ(1) (= −v(1) beam can be obtained by substituting z = 5000 mm in Eqs 9.13: εr(1) = u(1) (z = 5000) = −42.7 × 10−6 and κ(1) = −v(1) (z = 5000)

= 0.331 × 10−6 mm−1 which, as expected, corresponds to the same solution obtained in Example 5.1.

Stiffness method and ﬁnite-element modelling 361 The coefﬁcients deﬁning the expressions for the concrete internal axial force and moment are determined from Eqs A.57 and A.59: ac0(1) = −28.16 × 103 N ac1(1) = −6.701 Nmm−1 ac2(1) = 670.2 × 10−6 Nmm−2 bc0(1) = −66.96 × 103 Nmm bc1(1) = 15.65 × 103 N bc2(1) = −1.564 Nmm−1 Element 2 Similar to element 1, the terms describing the response of element 2 are calculated as: u(2) = uL(2) vL(2) vL(2) uR(2) vR(2) vR(2) = 156.2 × 10−3 3.494 0 − 312.5 × 10−3 0 − 1.138 × 10−3 p(2) = ku(2) + pF.m(2) T = 30 × 103 N 0 N 50 × 106 Nmm −30 × 103 N −20 × 103 N 0 Nmm 1(2) = 0 mm−2 C 2(2) = −331.3 × 10−9 mm−1 C 3(2) = 0 C 4(2) = 3.494 mm C 5(2) = −42.69 × 10−6 C 6(2) = −156.2 × 10−3 mm C The mid-span values of the strain variables (already calculated with element 1) could also have been determined with element 2 using the expressions of Eqs 9.13 at z = 0 mm.

9.4 Time analysis using AEMM When using the AEMM, deformations and stresses are calculated at two instants, immediately after loading at τ0 and after the effects of creep and shrinkage have taken place at τk . The instantaneous analysis at τ0 was presented in the previous section. The time analysis at time τk is outlined in the following. Creep and shrinkage effects are included in the stiffness analysis using equivalent nodal actions. As already discussed for the member loads, the set of equivalent nodal

362 Stiffness method and ﬁnite-element modelling actions to be used in the stiffness method correspond to the opposite of the reactions obtained when the supports of the element under consideration are assumed to be ﬁxed at both ends. The reactions produced by creep and shrinkage effects and by member loads are derived in Appendix A (Eqs A.66) and are reproduced below. ⎡

L2

⎤

ac2,0 ac1,0 L ⎢ ⎥ + + ac0,0 − Fe,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 a + a L L ⎢ ⎥ c1,0 c2,0 − Fe,0 − α3,k L − bc0,0 + bc2,0 ⎢ ⎥ ⎢ ⎥ 2 6 ⎥ pF.cr,k = ⎢ ⎢ ⎥ 2 ⎢ ⎥ a L L a c2,0 c1,0 ⎢ ⎥ Fe,0 + + ac0,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ −Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ 2 ac1,0 + ac2,0 L 5L ⎥ ⎣− ⎦ Fe,0 − α3,k L + bc0,0 + bc1,0 L + bc2,0 2 6 ⎤ ⎡ Ee,k Ac εsh,k ⎥ ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ ⎢− Ee,k Bc εsh,k ⎥ ⎥ pF.sh.k = ⎢ ⎥ ⎢ ⎢−Ee,k Ac εsh,k ⎥ ⎥ ⎢ ⎥ ⎢ 0 ⎦ ⎣ Ee,k Bc εsh,k ⎡ ⎤ ⎡ ⎤ 0 −L/2 ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ α3,k ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢Lα3,k /2⎥ pF.m,k = ⎢ ⎥p + ⎢ ⎥n ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ −L/2 ⎦ ⎣ −α3,k ⎦ L2 /12 Lα3,k /2

(9.15a)

(9.15b)

(9.15c)

where the constants α0,k , α1,k , α2,k , α3,k and α4,k are obtained from the cross-sectional rigidies at time τk using Eqs A.50a–e, respectively. The subscripts ‘m’, ‘cr’ and ‘sh’ used in pF.m,k , pF.cr,k and pF.sh,k indicate that the ﬁxed end reactions relate to either member loads, creep effects or shrinkage effects, respectively. The calculation at time τk of the cross-sectional rigidities RA,k , RB,k and RI,k required for input into Eqs A.50 has already been outlined in Chapter 5 for different types of cross-sections. The timedependent behaviour of concrete is represented by Ee,k and Fe,0 (given in Eqs 4.35 and 4.46), while εsh,k denotes the shrinkage strain. The coefﬁcients acj,0 and bcj,0 (with j = 0 to 2) that are necessary to deﬁne the expressions of the concrete internal actions are speciﬁed in Eqs A.57 and A.59.

Stiffness method and ﬁnite-element modelling 363 The time analysis can then be carried out by assembling the opposite of the vectors pF.m,k , pF.cr,k and pF.sh,k for each element into the loading vector of the structure, Pk , while using the cross-sectional properties calculated at τk in the determination of the stiffness coefﬁcients of Kk . When the unknown displacements and reactions are evaluated based on Eqs 9.9, the end actions of each element (i.e. member actions) can be obtained by combining the results of the stiffness analysis with those related to member loads, creep and shrinkage as follows: pk = kk uk + pF.m,k + pF.cr,k + pF.sh,k

(9.16)

The axial displacement uk and deﬂection vk can be calculated along the member axis using Eqs A.63 (repeated here for convenience): z3 2 1,k + α4,k n + β3,k z + C 6,k 5,k z + C uk = α2,k p + β2,k + α3,k C 6 2 3 2 z4 1,k z + C 2,k z + C 3,k z + C 4,k +C vk = α1,k p + β1,k 24 6 2

(9.17a) (9.17b)

where the constants αj,k (with j = 0 to 4) and βj,k (with j = 1 to 3) are given in 6,k are 1,k to C Eqs A.50 and A.64, respectively and the constants of integration C given in Eqs A.67. The strain diagram at any point along an element can be obtained by differentiating Eqs 9.17 to give: z2 1,k + α4,k n + β3,k z + C 5,k + α3,k C uk = α2,k p + β2,k 2 z2 1,k z + C 2,k +C vk = α1,k p + β1,k 2

(9.18a) (9.18b)

from which the stresses may be evaluated following the procedures illustrated in Chapter 5.

Example 9.2 The deﬂection at time τk and the variables deﬁning the strain diagram (εr,k and κk ) at mid-span of the simply-supported beam analysed in Example 9.1 are to be determined, as well as the actions resisted by the two elements. The applied loads are assumed to remain constant with time. The cross-sectional and material properties of the beam are those of the reinforced concrete section considered in Example 5.3. The analysis is to be carried out using the stiffness method assuming the same two elements and freedom numbering as adopted in Example 9.1. All units are in mm and N, unless noted otherwise. From Example 5.3: Ee,k = 9524 MPa Fe,0 = −0.333 ϕ(τk , τ0 ) = 2.5

364 Stiffness method and ﬁnite-element modelling χ (τk , τ0 ) = 0.65 εsh (τk ) = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4 RA,k = 2175 × 106 N RB,k = 273.7 × 109 Nmm RI,k = 113.2 × 1012 Nmm2 and from Example 5.1: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 As for Example 9.1: T UU,k = U1,k U2,k U3,k U4,k U5,k U6,k T T UK,k = U7,k U8,k U9,k = 0 0 0 T PU,k = P7,k P8,k P9,k From Eqs A.50: α0,k = 171.4 × 1021 N2 mm2 α1,k = 12.69 × 10−15 N−1 mm−2 α2,k = 1597 × 10−15 N−1 mm−1 α3,k = 125.8 mm α4,k = −459.7 × 10−12 N−1 The stiffness matrix for both elements 1 and 2 are identical and calculated at time τk as (Eq. 9.2a): ⎡ ⎤ 435.0 × 103 0 −54.74 × 106 −435.0 × 103 0 −54.74 × 106 ⎢ ⎥ 7.563 × 103 18.91 × 106 0 −7.563 × 103 18.91 × 106 ⎥ ⎢ ⎢ ⎥ 9 6 6 9 ⎢ 54.74 × 10 −18.91 × 10 24.62 × 10 ⎥ 69.92 × 10 ⎥ ke = ⎢ ⎢ ⎥ 435.0 × 103 0 −54.74 × 106 ⎥ ⎢ ⎢ ⎥ 3 6 ⎣ sym 7.563 × 10 −18.91 × 10 ⎦ 69.92 × 109

Stiffness method and ﬁnite-element modelling 365 The set of reactions required to account for the member load p = 4 N/mm and for shrinkage are (Eqs 9.15b and c): ⎡

⎤ 0

⎡

⎤ 0N

⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ −10 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎢−L /12⎥ ⎢−8.3 × 106 Nmm⎥ pF.m,k(1) = pF.m,k(2) = ⎢ ⎥p = ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ −L/2 ⎥ ⎢ −10 × 103 N ⎥ ⎣ ⎦ ⎣ ⎦ L2 /12 8.3 × 106 Nmm ⎤ ⎡ ⎤ ⎡ ⎡ ⎤ 6 N E A ε −1014 × 10 a c sh,k e,k sh,k ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ 0 ⎥ ⎢ ⎥ 0 0N ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ 6 ⎢−bsh,k ⎥ ⎢−Ee,k Bc εsh,k ⎥ ⎢ 99.78 × 10 Nmm ⎥ pF.sh,k(1) = pF.sh,k(2) = ⎢ ⎥=⎢ ⎥=⎢ ⎥ ⎥ ⎢ ⎢−a ⎥ ⎢− ⎥ 6 ⎢ sh,k ⎥ ⎢ Ee,k Ac εsh,k ⎥ ⎢ 1014 × 10 N ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ 0 ⎥ ⎢ ⎥ 0 N 0 ⎦ ⎣ ⎦ ⎣ ⎣ ⎦ −99.78 × 106 Nmm bsh,k Ee,k Bc εsh,k The vectors pF.cr,k(1) and pF.cr,k(2) need to be evaluated for the two elements separately. From Example 9.1: ac0(1),0 = −28.16 × 103 N ac1(1),0 = −6.701 Nmm−1 ac2(1),0 = 670.2 × 10−6 Nmm−2 bc0(1),0 = −66.96 × 103 Nmm bc1(1),0 = 15.65 × 103 N bc2(1),0 = −1.564 Nmm−1 ac0(2),0 = −44.91 × 103 N ac1(2),0 = 2.788 × 10−12 Nmm−1 ac2(2),0 = 670.2 × 10−6 Nmm−2 bc0(2),0 = 39.05 × 106 Nmm bc1(2),0 = −6.509 × 10−12 N bc2(2),0 = −1.564 Nmm−1

366 Stiffness method and ﬁnite-element modelling From Eq. 9.15a: ⎡

⎡ ⎤ ⎤ −13.11 × 103 N −13.11 × 103 N ⎢ ⎢ ⎥ ⎥ ⎢ 2.748 × 103 N ⎥ ⎢ −2.748 × 103 N ⎥ ⎢ ⎢ ⎥ ⎥ 6 ⎢−1.799 × 106 Nmm⎥ ⎢ ⎥ ⎥ and pF.cr(2),k = ⎢−15.54 × 10 Nmm⎥ pF.cr(1),k = ⎢ ⎢ 13.11 × 103 N ⎥ ⎢ 13.11 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ ⎣ −2.748 × 103 N ⎦ ⎣ 2.748 × 103 N ⎦ 15.54 × 106 Nmm 1.799 × 106 Nmm

After assembly, the sub-matrices of Kk and the loading vector Pk of the whole structure at τk are: ⎤ ⎡ 69.92 × 109 54.74 × 106 −18.91 × 106

⎢ ⎢ ⎢ ⎢ K11,k = ⎢ ⎢ ⎢ ⎢ ⎣ ⎡

870.1 × 103

⎢ K22,k = ⎢ ⎣

0

−109.5 × 106 −435.0 × 103

0 15.13 × 103

0

0

139.8 × 109

54.74 × 106 435.0 × 103

sym

−54.74 × 106

⎢ ⎢−435.0 × 103 ⎢ ⎢ ⎢ 0 K12,k = ⎢ ⎢ ⎢ 54.74 × 106 ⎢ ⎢ 0 ⎣ ⎡

24.63 × 109

0 435.0 × 103 sym

⎤

18.91 × 106

0

0

0

0

⎥ ⎥ 18.91 × 106 ⎥ ⎥ ⎥ 24.63 × 109 ⎥ ⎥ −54.74 × 106⎦ 54.74 × 106 ⎥

69.92 × 109

⎥ ⎥ ⎥ ⎥ 3 3 −7.56 × 10 −7.56 × 10 ⎥ ⎥ ⎥ 6 6 18.91 × 10 −18.91 × 10 ⎥ ⎥ ⎥ 0 0 ⎦ 6 0 −18.91 × 10 ⎤ 0 0 ⎥ ⎥ 7.563 × 103 0 ⎦ 7.563 × 103

T K21,k = K12,k

Pk = [89.66 × 106 0

25.50 × 103

0

−1057 × 103

89.66 × 106

(P7 + 1027 × 103 ) (P8 + 7.252 × 103 ) (P7 + 7.252 × 103 )]T

From Eqs 9.9, unknown displacements UU,k and reactions PU,k are obtained: ⎤ ⎡ 4.781 × 10−3 ⎥ ⎢ ⎢ −3.033 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ 13.65 mm ⎥ −1 UU,k = K11,k PK,k − K12,k UK,k = ⎢ ⎥ and ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ −6.066 mm ⎦ ⎣ −4.780 × 10−3

Stiffness method and ﬁnite-element modelling 367 ⎤ 30 × 106 N P7,k ⎥ ⎢ ⎢ ⎥ PU,k = ⎣P8,k ⎦ = ⎣−20 × 106 N⎦ ⎤

⎡

P9,k

⎡

−20 × 106 N

The mid-span deﬂection at τk (associated with freedom 3) is 13.65 mm which has increased from its initial value of 3.49 mm.

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element. Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: ⎤ ⎡ ⎡ ⎤ uL(1),k 0 mm ⎥ ⎢ ⎢ ⎥ ⎢ vL(1),k ⎥ ⎢ ⎥ 0 mm ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ v ⎥ −3 ⎢ L(1),k ⎥ ⎢4.781 × 10 ⎥ u(1),k = ⎢ ⎥=⎢ ⎥ ⎢uR(1),k ⎥ ⎢ −3.033 mm ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎣vR(1),k ⎦ ⎣ 13.65 mm ⎦ 0 vR(1),k p(1),k = kk u(1),k + pF.m(1),k + pF.cr(1),k + pF.sh(1),k T = 30 × 103 −20 × 103 0 −30 × 103 0 −50 × 106 As expected, the member actions are identical to the instantaneous values as the structure is statically determinate. From Eqs A.67: 1(1),k = −323.6 × 10−12 mm−2 C 2(1),k = −416.7 × 10−9 mm−1 C 3(1),k = 4.780 × 10−3 C 4(1),k = 0 mm C 5(1),k = −539.6 × 10−6 C 6(1),k = 0 mm C The axial strain measured at the level of the reference axis and the curvature at mid-span are determined by substituting the calculated constants of integration into Eqs 9.18 with z = 5000 mm: i.e. εr(1),k = u(1),k = −641.4 × 10−6 and κ(1),k =

= 1.225 × 10−6 mm−1 . As expected, these results are identical to those −v(1),k calculated in Example 5.3.

368 Stiffness method and ﬁnite-element modelling Element 2 The nodal displacements and the member actions associated with the end nodes of element 1 are: ⎤ −3.033 mm ⎥ ⎢ ⎥ ⎢ ⎢ vL(2),k ⎥ ⎢ 13.65 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ v 0 ⎥ ⎢ L(2),k ⎥ ⎢ u(2),k = ⎢ ⎥=⎢ ⎥ ⎢uR(2),k ⎥ ⎢ −6.066 mm ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 ⎦ ⎣vR(2),k ⎦ ⎣ −3 −4.780 × 10 vR(2),k ⎡

uL(2),k

⎤

⎡

p(2),k = kk u(1),k + pF.m(1),k + pF.cr(1),k + pF.sh(1),k = 30 × 103 0 50 × 106 −30 × 103 −20 × 103

T 0

9.5 Time analysis using SSM When using the SSM, the time domain is discretised into a number of time instants τi (with i = 1, . . . , k) as shown in Fig. 4.3. As for the AEMM discussed in the previous section, the time-dependent behaviour of the concrete is included in the analysis using equivalent nodal actions that correspond to the opposite of the reactions obtained when the ends of the element are ﬁxed and the member is loaded and subject to creep and shrinkage. These reactions are determined at a particular instant in time, here referred to as τk , and are expressed as the vectors pF.m,k , pF.cr,k and pF.sh,k in Eqs A.91. Most of the notation used in the expressions for pF.m,k , pF.cr,k and pF.sh,k has already been deﬁned in the previous section. The procedure for the SSM and the various constants and coefﬁcients are derived in the Section A.5.3 and presented in Eqs A.71– A.91. The loading vector Pk is assembled, including the contributions of pF.m,k , pF.cr,k and pF.sh,k for every element, and the stiffness coefﬁcients for Kk are calculated based on the cross-sectional rigidities determined at time τk . The solution at time τk is obtained using Eqs 9.9. Post-processing to obtain stresses and strains on particular cross-sections is as described previously. The element end actions are evaluated from Eq. 9.16 and the axial displacement and deﬂection at any distance z along the element are expressed by Eqs A.77. The variables describing the strain diagram at time τk (εr,k = uk and κk = −vk ) are obtained from Eqs A.80.

Example 9.3 The simply-supported beam analysed in Example 9.2 is to be re-analysed using the stiffness method and using the SSM to handle the time effects. The time domain is discretised into three time instants: τ0 = 28 days, τ1 = 100 days and τ2 = 30,000 days. The deﬂection and the axial strain at the level of the

Stiffness method and ﬁnite-element modelling 369 reference axis and curvature at mid-span are to be calculated at each of these time instants. In addition, the member actions at each time step are determined for both elements. As in Examples 9.1 and 9.2, two elements are considered with freedom numbering as shown in Fig. 9.5. The cross-section of the beam at mid-span was previously analysed using the SSM in Example 5.5, where: Ec,0 = 25 GPa Ec,1 = 28 GPa Ec,2 = 30 GPa Fe,1,0 = −1.8 Fe,2,0 = −0.986 Fe,2,1 = −2.214 εsh (τ0 ) = εsh,0 = 0 εsh (τ1 ) = εsh,1 = −300 × 10−6 εsh (τ2 ) = εsh,2 = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4 Similarly to Example 9.1, the sets of known and unknown displacements and unknown actions for the three time steps τj (with j = 1, 2, 3) are: T UU,j = U1,j U2,j U3,j U4,j U5,j U6,j T T UK,j = U7,j U8,j U9,j = 0 0 0 T PU,j = P7,j P8,j P9,j From Examples 5.1 and 5.5: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 RA,1 = 5456 × 106 N RB,1 = 596.4 × 109 Nmm RI,1 = 241.9 × 1012 Nmm2 RA,2 = 5811 × 106 N RB,2 = 631.3 × 109 Nmm RI,2 = 255.8 × 1012 Nmm2

370 Stiffness method and ﬁnite-element modelling From Eqs A.50: α0,1 = 792.3 × 1021 N2 mm2 α1,1 = 6.214 × 10−15 N−1 mm−2 α2,1 = 686.6 × 10−15 N−1 mm−1 α3,1 = 110.5 mm α4,1 = −203.1 × 10−12 N−1 α0,2 = 964.4 × 1021 N2 mm2 α1,2 = 5.658 × 10−15 N−1 mm−2 α2,2 = 618.4 × 10−15 N−1 mm−1 α3,2 = 109.3 mm α4,2 = −193.3 × 10−12 N−1

Short-term analysis (τ0 = 28 days) The solution at time τ0 is identical to that presented in Example 9.1.

Time analysis – SSM (τ1 = 100 days) The stiffness matrix for elements 1 and 2 is determined using Eq. 9.2a with the rigidities calculated at time τ1 : ⎡ ⎤ 1091 × 103 0 −119.3 × 106 −1091 × 103 0 119.3 × 106 ⎢ ⎥ ⎢ 16.97 × 103 42.42 × 106 0 −16.97 × 103 42.42 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ 9 6 6 9 ⎥ ⎢ 154.4 × 10 119.3 × 10 −42.42 × 10 57.66 × 10 ⎥ k1 = ⎢ ⎢ ⎥ ⎢ 1091 × 103 0 −119.3 × 106 ⎥ ⎢ ⎥ ⎢ sym 16.97 × 103 −42.42 × 106 ⎥ ⎣ ⎦ 154.4 × 109

Since, the external loads are constant in time, the sets of reactions required to account for the member load p = 4 N/mm (i.e. pF,m(1),1 and pF,m(2),1 ) are identical to those determined in Example 9.1 at τ0 . Shrinkage is accounted for using Eq. A.91b with ⎤ ⎡ ⎤ −1491 × 106 Ec,1 Ac εsh,1 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 6 ⎢−Ec,1 Bc εsh,1 ⎥ ⎢ 146.7 × 10 ⎥ pF.sh(1),1 = pF.sh(2),1 = ⎢ ⎥=⎢ ⎥ ⎢−Ec,1 Ac εsh,1 ⎥ ⎢ 1491 × 106 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎦ ⎣ ⎦ ⎣ ⎡

Ec,1 Bc εsh,1

−146.7 × 106

Stiffness method and ﬁnite-element modelling 371 From Example 9.1, for element 1: ac0(1),0 = −28.16 × 103 Nmm2 ac1(1),0 = −6.701 Nmm−1 ac2(1),0 = 670.2 × 10−6 Nmm−2 bc0(1),0 = −66.96 × 103 Nmm bc1(1),0 = 15.65 × 103 N bc2(1),0 = −1.564 Nmm−1 and for element 2: ac0(2),0 = −44.91 × 103 Nmm2 ac1(2),0 = 2.788 × 10−12 Nmm−1 ac2(2),0 = 670.2 × 10−6 Nmm−2 bc0(2),0 = 39.05 × 106 Nmm bc1(2),0 = −6.509 × 10−12 N bc2(2),0 = −1.564 Nmm−1 From Eq. A.91, the creep effects are included in pF,cr(1),1 and pF,cr(2),1 : ⎤ ⎤ ⎡ −70.8 × 103 −70.8 × 103 ⎥ ⎥ ⎢ ⎢ ⎢ 14.74 × 103 ⎥ ⎢−14.74 × 103 ⎥ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎢−9.968 × 106 ⎥ ⎢−83.67 × 106 ⎥ pF.cr(1),1 = ⎢ and pF.cr(2),1 = ⎢ ⎥ ⎥ ⎢ 70.8 × 103 ⎥ ⎢ 70.8 × 103 ⎥ ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎣−14.74 × 103 ⎦ ⎣ 14.74 × 103 ⎦ 83.67 × 106 9.968 × 106 ⎡

After assembly, the sub-matrices of K1 and the load vector P1 of the whole structure at τ1 are: ⎤

⎡ 154.4 × 109 119.3 × 106 −42.42 × 106

⎢ ⎢ ⎢ ⎢ K11,1 = ⎢ ⎢ ⎢ ⎢ ⎣

2182 × 103

0 119.3 × 103

sym

57.66 × 109

0

−238.5 × 106 −1091 × 103 0

0

308.9 × 109

119.3 × 106 1091 × 103

0

⎥ ⎥ 42.42 × 106⎥ ⎥ ⎥ 57.66 × 109⎥ ⎥ −119.3 × 106⎦ 119.3 × 106⎥

154.4 × 109

372 Stiffness method and ﬁnite-element modelling ⎡ 0 −119.3 × 106 42.42 × 106 ⎢ ⎢ −1091 × 103 0 0 ⎢ ⎢ 3 ⎢ 0 −16.97 × 10 −16.97 × 103 K12,1 = ⎢ ⎢ ⎢ 119.3 × 106 42.42 × 106 −42.42 × 106 ⎢ ⎢ 0 0 0 ⎣ 0 0 −42.42 × 106 ⎡ ⎤ 0 0 1091 × 103 ⎢ ⎥ K22,1 = ⎣ ⎦ 16.97 × 103 0

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦

16.97 × 103

sym T K21,1 = K12,1

P1 = − 128.4 × 106 0

49.48 × 103 0 −1592 × 103 128.4 × 106 T (P7 + 1562 × 103 ) (P8 − 4.742 × 103 ) (P7 − 4.742 × 103 )

Solving for the unknown displacements and reactions using Eqs 9.9 gives: ⎤ ⎡ 3.042 × 10−3 ⎥ ⎢ ⎥ ⎢ −1.792 ⎥ ⎢ ⎥ ⎢ ⎢ 9.063 ⎥ −1 UU,1 = K11,1 PK,1 − K12,1 UK,1 = ⎢ ⎥ ⎥ ⎢ 0 ⎥ ⎢ ⎥ ⎢ −3.583 ⎦ ⎣ −3 −3.042 × 10 ⎤ ⎡ ⎤ ⎡ 30 × 106 P7,1 ⎥ ⎢ ⎥ ⎢ PU,1 = ⎣P8,1 ⎦ = ⎣−20 × 106 ⎦ P9,1

−20 × 106

Post-processing The solution is post-processed below to determine the variables deﬁning the strain diagram and the internal actions along each element. Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: T u(1),1 = 0 0 3.042 × 10−3 −1.792 9.063 0 p(1),1 = k1 u(1),1 + pF.m(1),1 + pF.cr(1),1 + pF.sh(1),1 T = 30 × 103 −20 × 103 0 −30 × 103 0 −50 × 106

Stiffness method and ﬁnite-element modelling 373 Using Eqs A.90: β1(1),1 = 33.36 × 10−15 mm β2(1),1 = 4.088 × 10−12 mm2 β3(1),1 = −2.211 × 10−9 mm−1 From Eqs A.79: 1(1),1 = −280 × 10−12 mm−2 C 2(1),1 = −141.7 × 10−9 mm−1 C 3(1),1 = 3.042 × 10−3 C 4(1),1 = 0 mm C 5(1),1 = −303.7 × 10−6 C 6(1),1 = 0 mm C The axial strain and curvature are calculated at mid-span by substituting z = 5000 mm into Eqs A.68 giving εr(1),1 = u(1),1 = −385.7 × 10−6 and κ(1),1 = = 0.841 × 10−6 mm−1 , which are the same as the results of Example 5.5 −v(1),1 at τ1 . From Eqs A.82 and A.84: ac0(1),1 = 101.7 × 103 Nmm2 ac1(1),1 = −14.19 Nmm−1 ac2(1),1 = 1419 × 10−6 Nmm−2 bc0(1),1 = 25.97 × 106 Nmm bc1(1),1 = 10.39 × 103 N bc2(1),1 = −1.039 Nmm−1 Element 2 T u(2),1 = −1.792 9.063 0 −3.583 0 −3.042 × 10−3 T p(2),1 = 30 × 103 0 50 × 106 −30 × 103 −20 × 103 0

374 Stiffness method and ﬁnite-element modelling

Time analysis – SSM (τ2 = 30,000 days) Following the procedure outlined for the time analysis at τ1 , the stiffness matrix for elements 1 and 2 is based on the rigidities at τ2 : ⎡ ⎤ 1162 × 103 0 −126.3 × 106 −1162 × 103 0 126.3 × 106 ⎢ ⎥ ⎢ ⎥ 17.97 × 103 44.95 × 106 0 −17.98 × 103 44.95 × 106 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ 163.5 × 109 126.3 × 106 −44.95 × 106 61.19 × 109 ⎥ k2 = ⎢ ⎢ ⎥ ⎢ 1162 × 103 0 −126.3 × 106 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ sym 19.97 × 103 −44.95 × 106 ⎥ ⎣ ⎦ 163.5 × 109

The equivalent nodal loads to account for shrinkage and creep in each element are: ⎤ ⎡ ⎤ ⎡ −3196 × 106 Ec,2 Ac εsh,2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 6 ⎢−Ec,2 Bc εsh,2 ⎥ ⎢ 314.3 × 10 ⎥ pF.sh(1),2 = pF.sh(2),2 = ⎢ ⎥=⎢ ⎥ ⎢−Ec,2 Ac εsh,2 ⎥ ⎢ 3196 × 106 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 0 0 ⎦ ⎣ ⎦ ⎣ 6 Ec,2 Bc εsh,2 −314.3 × 10 ⎤ ⎡ 134.2 × 103 ⎥ ⎢ ⎢ 21.29 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢−68.29 × 106 ⎥ pF.cr(1),2 = ⎢ ⎥ ⎢−134.2 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎣−21.29 × 103 ⎦ 174.7 × 106 ⎤ ⎡ 134.2 × 103 ⎥ ⎢ ⎢−21.29 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎢−174.7 × 106 ⎥ pF.cr(2),2 = ⎢ ⎥ ⎢−134.2 × 103 ⎥ ⎥ ⎢ ⎥ ⎢ ⎣ 21.29 × 103 ⎦ 68.3 × 106 Assembling of the stiffness matrix K2 and load vector P2 for the whole structure: ⎡

162.5 × 109 126.3 × 106 −44.95 × 106

⎢ ⎢ ⎢ ⎢ K11,2 = ⎢ ⎢ ⎢ ⎣

2324 × 103

0 35.96 × 103

sym

61.19 × 109

⎤ 0

−252.5 × 106 −1162 × 103 0

0

327.1 × 109

126.3 × 106 1162 × 103

0

⎥ ⎥ ⎥ 44.95 × 106 ⎥ ⎥ 61.19 × 109 ⎥ ⎥ −126.3 × 106 ⎦ 126.3 × 106

163.5 × 109

⎡

−126.3 × 106 ⎢ ⎢ −1162 × 103 ⎢ ⎢ ⎢ 0 K12,2 = ⎢ ⎢ ⎢ 126.3 × 106 ⎢ ⎢ 0 ⎣ 0 ⎡ ⎢ K22,2 = ⎢ ⎣

Stiffness method and ﬁnite-element modelling 375 ⎤ 44.95 × 106 0 ⎥ ⎥ 0 0 ⎥ ⎥ −17.98 × 103 −17.98 × 103 ⎥ ⎥ ⎥ 44.95 × 106 −44.95 × 106 ⎥ ⎥ ⎥ 0 0 ⎦ 0 −44.95 × 106 ⎤

1162 × 103

0

0

17.98 × 103

0

⎥ ⎥ ⎦

17.98 × 103

sym T K21,2 = K12,2

P2 = − 237.7 × 106

0

62.57 × 103

−3092 × 103

0

(P7 + 3062 × 103 )

(P8 − 11.29 × 103 )

237.7 × 106

T (P7 − 11.29 × 103 )

Solving for the unknown displacements and reactions using Eqs 9.9 gives: ⎡ ⎢ ⎢ ⎢ ⎢ ⎢ −1 UU,2 = K11,2 PK,2 − K12,2 UK,2 = ⎢ ⎢ ⎢ ⎢ ⎢ ⎣

4.71 × 10−3 −3.172 13.51 0 −6.344 −4.71 × 10−3

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ and ⎥ ⎥ ⎥ ⎥ ⎦

⎤ ⎤ ⎡ 30 × 106 P7,2 ⎥ ⎥ ⎢ ⎢ 6⎥ PU,2 = ⎣P8,2 ⎦ = ⎢ ⎣−20 × 10 ⎦ ⎡

−20 × 106

P9,2

Post-processing: Element 1 The nodal displacements and the member actions associated with the end nodes of element 1 are: u(1),2 = 0

0

4.71 × 10−3

p(1),2 = 30 × 103

−20 × 103

−3.172

13.51

0 −30 × 103

T 0 0 −50 × 106

T

376 Stiffness method and ﬁnite-element modelling and with: β1(1),2 = 45.46 × 10−15 mm β2(1),2 = 6.247 × 10−12 mm2 β3(1),2 = −6.542 × 10−9 mm−1 1(1),2 = −334.1 × 10−12 mm−2 C 2(1),2 = −385.1 × 10−9 mm−1 C 3(1),2 = 4.71 × 10−3 C 4(1),2 = 0 mm C 5(1),2 = −563.0 × 10−6 C 6(1),2 = 0 mm C The axial strain and curvature calculated at mid-span (i.e. at z = 5000 mm) at τ2 are: εr(1),2 = u(1),2 = −385.7 × 10−6 and κ(1),2 = −v(1),2 = 0.841 × 10−6 mm−1

Element 2 T u(2),2 = −3.172 13.51 0 −6.344 0 −4.71 × 10−3 T p(2),2 = 30 × 103 0 50 × 106 −30 × 103 −20 × 103 0

9.6 Time analysis using the ﬁnite-element method The ﬁnite-element method is a well-established method of analysis extensively used in all disciplines of engineering and its use is well reported in the literature (Ref. 2). Only the main aspects related to this method are outlined here, with particular attention placed on how time effects can be included in the analysis. For illustrative purposes, a displacement-based line element similar to the one described for the stiffness method is considered in the following. Its detailed formulation is outlined in Appendix A. The proposed approach for the inclusion of time effects in ﬁnite-element analysis can be extended to any other type of ﬁnite element, i.e. displacement-based, force-based or mixed elements. For ease of notation, subscripts deﬁning particular time instants are included only when the instant considered is not clear from the context. The weak form of the problem used to derive the proposed line ﬁnite element is obtained by means of the principle of virtual work as outlined in Section A.3. Restating Eq. A.18: ri · A eˆ dz = q · eˆ dz (9.19) L

L

Stiffness method and ﬁnite-element modelling 377 in which q contains the external distributed loads n and p (Fig. 9.3) and the vector e contains the independent variables deﬁning the displacement ﬁeld for the Euler– Bernoulli beam model consisting of the axial displacement measured at the level of the reference axis u and the deﬂection v. That is: n q= (9.20a) p u e= (9.20b) v The variables deﬁning the strain diagram, i.e. εr and κ, are obtained by differentiating e as follows (Eq. A.16): εr u ε= = = Ae (9.21) κ −v where the differential operator A is expressed (with ∂ ≡

∂ 0 A= 0 −∂ 2

d (·) ) by: dz

and the expression for the axial strain at a point in the member ε is: ε = εr + yκ = u − yv = 1 y ε

(9.22)

(9.23)

The internal resultants collected in ri (i.e. the internal axial force and moment) have been deﬁned in Chapter 5 for different types of cross-sections and may be expressed as (Eqs A.11): ri = Dε + fcr − fsh

(9.24)

where the terms related to creep and shrinkage vanish when performing an instantaneous analysis. The vectors and matrices in Eq. 9.24 are expanded in Eqs A.13 (and were used in Chapters 5 and 7). The vectors f cr and f sh depicting the creep and shrinkage response have been expressed in terms of their components fcrN , fcrM , fshN , and fshM to simplify the notation and, for the AEMM, are given by Eqs A.14 and, for the SSM, are given in Eqs A.15. The proposed ﬁnite-element formulation relies on the approximation of the independent variables deﬁning the kinematic response, i.e. u and v previously collected in e (Eq. 9.20b), as follows: e ≈ N e de

(9.25)

where de are the nodal displacements of the ﬁnite element under consideration and Ne contains the shape functions that describe the variations of these displacements along the element length.

378 Stiffness method and ﬁnite-element modelling Similarly to the stiffness relationship of Eq. 9.1, the governing system of equations describing the behaviour of a line element can be expressed in terms of nodal displacements de and actions pe : pe = ke de

(9.26)

where ke is the ﬁnite element stiffness matrix (given in Eq. A.25a and reproduced here as Eq. 9.27) and pe is the load vector accounting for the contributions of pe.m , pe.cr , and pe.sh (given in Eqs A.25b and A.26): ke =

T

L

(A Ne ) D ε dz =

L

(A Ne )T D (A Ne ) dz

(9.27)

The derivation for a particular ﬁnite element is carried out here for the 7 DOF element depicted in Fig. 9.6. In this case the axial and vertical displacements are approximated by parabolic and cubic polynomials, respectively. The nodal displacements and shape functions expressing this approximation are outlined in Eqs A.27–A.30 and the stiffness matrix and load vector related to member loads n and p are given in Eqs A.31 and A.32 (reproduced below): ⎡ −4RB −3RB −8RA RA ⎢ 7RA ⎢ 3L 2 L 3L 3L L ⎢ ⎢ ⎢ −4RB 12RI 6RI 8RB −4RB ⎢ ⎢ L2 L3 L2 L2 L2 ⎢ ⎢ ⎢ −3RB 6RI 4RI 4RB −RB ⎢ ⎢ 2 L L L L ⎢ L ⎢ ⎢ −8R 4RB 8RB 16RA −8RA ke = ⎢ A ⎢ 2 ⎢ 3L L 3L 3L L ⎢ ⎢ R −4RB −RB −8RA 7RA ⎢ A ⎢ 2 ⎢ 3L L 3L 3L L ⎢ ⎢ −12RI −6RI −8RB 4RB ⎢ 4RB ⎢ 3 2 2 ⎢ L2 L L L L2 ⎢ ⎣ −RB 6RI 2RI 4RB −3RB L L L L L2

T L L L2 2L L L L2 pe.m = n p p n n p − p 6 2 12 3 6 2 12 qR uM

uL

qL vL

4RB L2 −12RI L3 −6RI L2 −8RB L2 4RB L2 12RI L3 −6RI L2

⎤ −RB ⎥ L ⎥ ⎥ ⎥ 6RI ⎥ ⎥ L2 ⎥ ⎥ ⎥ 2RI ⎥ ⎥ ⎥ L ⎥ ⎥ 4RB ⎥ ⎥ (9.28) ⎥ L ⎥ ⎥ −3RB ⎥ ⎥ ⎥ L ⎥ ⎥ ⎥ −6RI ⎥ ⎥ L2 ⎥ ⎥ ⎦ 4RI L

uR

vR

z L

Figure 9.6 Nodal displacements of the 7 DOF ﬁnite element.

(9.29)

Stiffness method and ﬁnite-element modelling 379 For illustrative purposes and to better outline all the steps involved in the solution process, the integrals in the expressions for ke (Eq. 9.27) and pe.m (Eq. A.26a) have been solved analytically throughout this chapter and in Appendix A. However, numerical integration could be easily implemented if preferred. Even if not carried out in the following, static condensation could be used to handle the internal freedom (Ref. 2). The stiffness relationship of Eq. 9.26 is expressed in the local coordinates of the member (assuming the z-axis coincides with the member axis). This relationship must be transformed and expressed in global coordinates (i.e. coordinate system applicable to the whole structure) following the procedure previously outlined for the stiffness method in Eqs 9.3–9.6. The transformation matrix T for the 7 DOF ﬁnite element is: ⎡

c

s

⎢ ⎢−s c ⎢ ⎢ ⎢0 0 ⎢ T=⎢ ⎢0 0 ⎢ ⎢0 0 ⎢ ⎢ ⎣0 0 0

0 0

0

0 0

0

1 0

0

0 1

0

0

0

c

0

0 −s

0 0 0

0

⎤ 0 0 ⎥ 0 0⎥ ⎥ ⎥ 0 0⎥ ⎥ 0 0⎥ ⎥ ⎥ s 0⎥ ⎥ ⎥ c 0⎦

(9.30)

0 1

The assembly procedure required to yield the stiffness relationship applicable to the whole structure is similar to the one utilised for the stiffness method. This produces relationships similar to those already presented in Eqs 9.7 and 9.8. The unknown displacements and reactions can be solved using Eqs 9.9. When the analysis is completed, the solution is post-processed and, for each element, the different variables describing its structural response are determined. For example, the variables deﬁning the strain diagram can be obtained by substituting the approximated displacements (Eq. 9.25) into Eq. 9.21 (Eqs A.34):

3 4 1 4 8 4 u = − uL + uM − uR + z (9.31a) u − u + u L M R L L L L2 L2 L2

6 4 6 2 12 6 12 6 v = − 2 v L − θL + 2 v R − θR + vL + 2 θL − 3 vR + 2 θR z (9.31b) L L L L L3 L L L where all nodal displacements are deﬁned in Fig. 9.6. Considering the post-processing of the instantaneous analysis, the stress resultants resisted by the concrete component can be expressed as (Eqs A.35a and d): Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0 = ac0,0 + ac1,0 z

(9.32a)

Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0

(9.32b)

= bc0,0 + bc1,0 z

where the adopted subscript ‘0’ has been introduced to highlight that these expressions are only applicable at time τ0 . The coefﬁcients ac0,0 , ac1,0 , bc0,0 and bc1,0 are given in Eqs A.35.

380 Stiffness method and ﬁnite-element modelling As previously mentioned, for the calculation of the terms in ke and pe.m (Eqs 9.28 and 9.29) numerical integration could be used. For example, the axial force and moment resisted by the concrete at τ0 could be calculated by numerical integration of the expressions presented in Eqs A.33. For clarity, an approach similar to the one already presented for the stiffness method has been adopted in which the variables are represented using polynomials that, in this case, are linear for both Nc,0 and Mc,0 (Eqs 9.32). Obviously, numerical integration could be easily implemented if preferred in the proposed solution process. The use of the linear polynomial has been determined by considering the degree of the polynomials adopted to approximate the displacements u and v in Eqs A.27–A.29. Based on these the variations of both u and v deﬁning the strain diagram (Eq. 9.31) are linear functions of z and, as a consequence, so to are the expressions for Nc,0 and Mc,0 in Eqs 9.32. 9.6.1 Load vector to account for time effects using the AEMM The calculation of the loading vector describing creep effects, i.e. pe.cr introduced in Eq. A.26b, requires the knowledge of the axial force fcrN and moment fcrM included in f cr which, when considering the AEMM, is deﬁned in Eqs A.14a and c. Both fcrN and fcrM are found by multiplying the axial force and moment resisted by the concrete at time τ0 by the material coefﬁcient Fe,0 : fcrN = Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z

(9.33a) (9.33b)

Equations 9.33 highlight that it is necessary to record the stress state of the concrete obtained from the instantaneous analysis before initiating the time analysis. When using numerical integration for the calculation of the stress resultants in the concrete, the values of the concrete axial force and moment at particular locations at time τ0 along each member are stored. These locations are usually those required by the numerical integration of Eqs A.25 and A.27. Another option, used in the following (and in Appendix A), is to identify polynomials capable of describing the variations of the concrete axial force and moment along each element and to store the relevant coefﬁcients. This has already been carried out in Eqs 9.32. The loading vector describing shrinkage effects pe.sh is expressed as Eq. A.26c. If it assumed that the shrinkage of a member does not vary along its length, the axial force fshN and moment fshM required to deﬁne f sh in Eq. A.26c are given by: fshN =

Ac

fshM =

Ac

Ee,k εsh,k dA = Ee,k Ac εsh,k

(9.34a)

y Ee,k εsh,k dA = Ee,k Bc εsh,k

(9.34b)

Based on the expressions for fcrN and fcrM (Eqs 9.33) and fshN and fshM (Eqs 9.34) and the deﬁnitions of pe.cr and pe.sh (Eqs A.26b and c), it is possible to determine the load vectors which account for creep and shrinkage. These are derived in Appendix A and given in Eqs A.36 and A.37.

Stiffness method and ﬁnite-element modelling 381 9.6.2 Load vector to account for time effects using the SSM Assuming the time-dependent behaviour of the concrete to be modelled by means of the SSM the expressions for fcrN and fcrM to be included in f cr are (Eqs A.15): fcrN =

fcrM =

k−1 i=0 Ac k−1 i=0 Ac

Fe,k,i σc,i dA =

k−1

Fe,k,i Nc,i

(9.35a)

i=0

yFe,k,i σc,i dA =

k−1

Fe,k,i Mc,i

(9.35b)

i=0

where the variation of the concrete stress resultants has also been described by a linear polynomial. For any time τi , the axial force and moment resisted by the concrete is calculated using the linear polynomials as given in Eqs A.41. Substituting the polynomial describing the variations of Nc,i and Mc,i expressed in Eqs A.41 into Eqs 9.35 gives: k−1

fcrN,k =

Fe,k,i Nc,i =

i=0 k−1

fcrM,k =

i=0

k−1

Fe,k,i ac0,i + ac1,i z

(9.36a)

Fe,k,i bc0,i + bc1,i z

(9.36b)

i=0

Fe,k,i Mc,i =

k−1 i=0

and the load vector accounting for creep is given as Eq. A.42. Similar to the inclusion of shrinkage effects in the AEMM, shrinkage is here included using: fshN = Ec,k εsh,k dA = Ec,k Ac εsh,k (9.37a) Ac

fshM =

Ac

yEc,k εsh,k dA = Ec,k Bc εsh,k

(9.37b)

9.6.3 Remarks on the consistency requirements for ﬁnite elements The proposed 7 DOF ﬁnite element represents the simplest element that fulﬁls the consistency requirements approximating the displacements by means of polynomials and thereby avoids potential locking problems which may arise when the member local z-axis does not pass through the centroid of the member cross-section (Refs 5 and 7). The ability to select a reference system with the origin not necessarily coincident with the centroid of the section is fundamental when dealing with time effects as the location of the actual centroid of a reinforced cross-section usually varies with time due to creep of the concrete. From a practical viewpoint, the consistency requirement is satisﬁed when the independent displacements (or their derivatives) present in the expressions of the strains of the model possess the same order (i.e. u and v have the same order). Adopting a cubic function for the deﬂection v produces a linear contribution to the

382 Stiffness method and ﬁnite-element modelling strain (i.e. due to v ). In order to produce the same (linear) contribution to the strain from u , it is necessary to have a parabolic function approximating the axial displacement u. For example, a linear function for u would not be able to achieve this as its ﬁrst derivative (i.e. u ) is constant. Other approaches could be used to address this problem, such as reduced integration. To better illustrate this behaviour, the results obtained using the 7 DOF ﬁnite element (Fig. 9.6) are compared to those calculated using a 6 DOF element (Fig. 9.7). The 6 DOF element approximates u and v by means of linear and cubic polynomials, respectively. As previously discussed, this latter element does not satisfy the consistency requirements due to the orders of its polynomials. The stiffness matrix of the 6 DOF ﬁnite element is: ⎤ ⎡ R R R R A B A B ⎥ ⎢ 0 − − 0 ⎢ L L L L ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ 12RI 6RI 12RI 6RI ⎥ ⎥ ⎢ 0 0 − 3 ⎥ ⎢ L3 L2 L L2 ⎥ ⎢ ⎥ ⎢ ⎢ R 6RI 4RI RB 6RI 2RI ⎥ ⎥ ⎢− B − 2 ⎥ ⎢ L L L L ⎥ L2 L (9.38) ke = ⎢ ⎥ ⎢ ⎥ ⎢ R RB RA RB ⎥ ⎢ A 0 0 − ⎥ ⎢− ⎢ L L L L ⎥ ⎥ ⎢ ⎢ 12RI 6RI 12RI 6RI ⎥ ⎥ ⎢ − 3 − 2 0 − 2 ⎥ ⎢ 0 3 ⎥ ⎢ L L L L ⎥ ⎢ ⎦ ⎣ RB 6RI 2RI RB 4RI 6RI − − L L L L L2 L2 For the case of an uncracked, simply supported, prismatic, concrete beam of rectangular section and subjected to a point load applied at mid-span, the instantaneous mid-span deﬂections calculated using the 6 and 7 DOF ﬁnite elements are shown in Fig. 9.8. These results have been obtained by considering two elements to clearly emphasise the implications of the different sets of polynomials. The instantaneous midspan deﬂection has been plotted for different levels of the reference axis dref (measured from the top of the section) expressed as a function of the depth D. With this notation the reference axis is located at the level of the centroid when dref /D = 0.5, in which case both elements produce the same mid-span deﬂection (noted as vmax in Fig. 9.8). Based on Fig. 9.8, it is apparent that when using the 6 DOF element with the origin of the reference system not coinciding with the cross-sectional centroid, a stiffer response than expected is obtained. A discussion on consistency requirements for different line elements is presented in Ref. 8. qR uL

qL vL

uR

vR

z L

Figure 9.7 Nodal displacements of the 6 DOF ﬁnite element.

Stiffness method and ﬁnite-element modelling 383

10%

vmax − vL/2 vmax [%]

8%

6 DOF element

6% 4% 2%

7 DOF element

dref D

0% 2

0

4

6

8

10

Figure 9.8 Comparisons between the results obtained using the 6 and 7 DOF ﬁnite elements.

Example 9.4 The short- and long-term values for the moment reaction at the ﬁxed support and the vertical reactions at the roller support of the propped cantilever shown in Fig. 9.9 are to be determined. The member is subjected to a point load applied at mid-span as shown. The time-dependent behaviour of the concrete is to be modelled using the AEMM and the cross-sectional and material properties are the same as in Example 5.3. For ease of notation, the beam is modelled using two of the 7 DOF line elements depicted in Fig. 9.6. 10 kN

B

1

2

A 10 m

C

10 m

Figure 9.9 Loading, support conditions and discretisation for Example 9.4.

The numbering of the freedoms adopted in the proposed solution is outlined in Fig. 9.10. The numbering system has been selected to produce the partitioning introduced in Eqs 9.8 and also to avoid the need for transformations from local to global coordinates (as the local and global coordinate axes coincide for each element). 1 10

2 C

B

A 9 11

7

2

1 3

4

8

5 6

Figure 9.10 Freedom numbering for Example 9.4.

384 Stiffness method and ﬁnite-element modelling From Examples 5.1 and 5.3: RA,0 = 4923 × 106 N RB,0 = 543.9 × 109 Nmm RI,0 = 221.0 × 1012 Nmm2 RA,k = 2175 × 106 N RB,k = 273.7 × 109 Nmm RI,k = 113.2 × 1012 Nmm2 Ec,0 = 25,000 MPa Ee,k = 9524 MPa Fe,0 = −0.333 ϕ(τk , τ0 ) = 2.5 χ(τk , τ0 ) = 0.65 εsh (τk ) = −600 × 10−6 Ac = 177.6 × 103 mm2 Bc = 17.46 × 106 mm3 Ic = 6966 × 106 mm4

Instantaneous analysis (at time τ0 ) Based on Fig. 9.10, freedoms 1–7 are unrestrained, while no displacement is permitted for each of freedoms 8–11. Therefore: T UU,0 = U1,0 U2,0 U3,0 U4,0 U5,0 U6,0 U7,0 T T UK,0 = U8,0 U9,0 U10,0 U11,0 = 0 0 0 0 T PU,0 = P8,0 P9,0 P10,0 P11,0 The ﬁnite-element stiffness matrix ke,0 is identical for both elements 1 and 2 and is calculated at time τ0 substituting RA,0 , RB,0 and RI,0 into Eq. 9.28 and specifying an element length L equal to 10 × 103 mm. The stiffness matrix of the whole structure is then assembled following similar steps to those carried out in previous examples. The unknown displacements and reactions are calculated using Eqs 9.9: ⎡ ⎤ 0.021 mm ⎢ ⎥ ⎤ ⎡ ⎡ ⎤ ⎢ 4.531 mm ⎥ ⎢ ⎥ −3125 N P8,0 −6 ⎢ 194.2 × 10 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ P9,0 ⎥ ⎢ 0N ⎥ ⎥ and PU,0 = ⎢ UU,0 = ⎢ = ⎥ ⎢ ⎢ ⎥ −0.059 mm ⎢ ⎥ ⎣P10,0 ⎦ ⎣ ⎦ −6875 N ⎢ ⎥ ⎢ −0.085 mm ⎥ 6 ⎢ ⎥ −37.5 × 10 Nmm P11,0 ⎣−776.7 × 10−6 ⎦ 0.070 mm

Stiffness method and ﬁnite-element modelling 385 The moment reaction at the ﬁxed support (related to freedom 11) and the vertical reaction at the roller support (related to freedom 8) are equal to −37.5 kNm and −3125 N, respectively.

Post-processing The solution is now post-processed to determine the coefﬁcients describing the variation of the concrete stress resultants required subsequently to account for creep effects. The nodal displacements for elements 1 and 2 at time τ0 are collected in vectors u(1),0 and u(2),0 : ⎡

⎤

uL(1),0

⎡

0 mm

⎤

⎤

⎡ uL(2),0

⎡

0.021 mm

⎥ ⎥ ⎢ ⎢ ⎥ ⎢vL(1),0⎥ ⎢ ⎢ vL(2),0 ⎥ ⎢ ⎥ 0 mm 4.531 mm ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎢ ⎥ ⎢ 194.2 × 10−6 v ⎥ ⎢vL(1),0⎥ ⎢ ⎢ 0 ⎥ ⎥ ⎢ ⎢ ⎢ L(2),0 ⎥ ⎢ ⎥ = ⎢ 0.070 mm ⎥ ⎥ ⎢ −0.059 mm ⎢u u(1),0 = ⎢ and u = ⎥ u (2),0 ⎢ M(1),0⎥ ⎢ ⎢ M(2),0 ⎥ = ⎢ ⎥ ⎥ ⎥ ⎢ ⎢ ⎢ ⎢uR(1),0⎥ ⎢ ⎢ uR(2),0 ⎥ ⎢ −0.085 mm 0.021 mm ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎢ ⎥ ⎣ 4.531 mm ⎥ ⎥ ⎢ ⎢v ⎢v ⎦ ⎣ 0 mm ⎣ R(1),0⎦ ⎣ R(2),0 ⎦ vR(1),0

194.2 × 10−6

vL(2),0

⎤ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎥ ⎦

−776.7 × 10−6

and from Eqs A.35: ac0(1),0 = 12.56 × 103 Nmm2 ac1(1),0 = −2.304 Nmm−1 bc0(1),0 = −29.34 × 106 Nmm bc1(1),0 = 5.379 × 103 N ac0(2),0 = −10.47 × 103 Nmm2 ac1(2),0 = 1.047 Nmm−1 bc0(2),0 = 24.45 × 106 Nmm bc1(2),0 = −2.45 × 103 N

Long-term analysis (at time τk ) The unknown and known displacements at time τk and the unknown reactions are: T UU,k = U1,k U2,k U3,k U4,k U5,k U6,k U7,k T T UK,k = U8,k U9,k U10,k U11,k = 0 0 0 0 T PU,k = P8,k P9,k P10,k P11,k

386 Stiffness method and ﬁnite-element modelling The ﬁnite-element stiffness matrix ke,k for elements 1 and 2 is obtained from Eq. 9.28 using the cross-sectional properties RA,k , RB,k and RI,k . The load vectors accounting for shrinkage effects for both elements 1 and 2 are calculated at time τk using Eq. A.37: ⎡ ⎤ 1015 × 103 N ⎢ ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎢−99.79 × 106 Nmm⎥ ⎢ ⎥ ⎢ ⎥ pe.sh(1),k = pe.sh(2),k = ⎢ ⎥ 0N ⎢ ⎥ ⎢ −1015 × 103 N ⎥ ⎢ ⎥ ⎢ ⎥ ⎣ ⎦ 0N 99.79 × 106 Nmm The vectors describing the creep effects for elements 1 and 2 are calculated from Eq. A.36 using the coefﬁcient acj(i),0 and bcj(i),0 stored at the end of the instantaneous analysis: ⎤ ⎡ ⎡ ⎤ 2909 N −2909 N ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ 1793 N −815.0 N ⎥ ⎢ ⎢ ⎥ ⎢9779 × 103 Nmm⎥ ⎢−8150 × 103 Nmm⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ pe.cr(1),k = ⎢ ⎥ ⎥ and pe.cr(2),k = ⎢ −5119 N 2327 N ⎥ ⎢ ⎢ ⎥ ⎢ ⎢ ⎥ ⎥ 2211 N 581.7 N ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎦ ⎣ ⎣ ⎦ −1793 N 815.0 N 8150 × 103 Nmm

0 Nmm

The unknown displacements and reaction are then obtained using Eqs 9.9 following assembly of the global stiffness matrix and load vector (as was previously carried out at time τ0 ): ⎡ ⎤ −4.544 mm ⎢ ⎥ ⎤ ⎡ ⎡ ⎤ ⎢ 19.22 mm ⎥ ⎢ ⎥ −1033 N P 8,k ⎢ 948.3 × 10−6 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ P9,k ⎥ ⎢ ⎥ 0N ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ UU,k = ⎢ −7.219 mm ⎥ and PU,k = ⎢ =⎢ ⎥ ⎥ ⎢ ⎥ −8967 N P ⎦ ⎣ ⎣ ⎦ 10,k ⎢ −9.814 mm ⎥ ⎢ ⎥ 6 −79.35 × 10 Nmm P11,k ⎢ ⎥ ⎣−3.793 × 10−3 ⎦ −2.051 mm The moment reaction at the ﬁxed support (related to freedom 11) and the vertical reaction at the roller support (related to freedom 8) are equal to −79.35 kNm and −1033 N, respectively. For this lightly loaded member, the preponderance of reinforcement in the bottom ﬁbres has caused the redistribution of internal actions illustrated in Fig. 8.5b(i).

Stiffness method and ﬁnite-element modelling 387

9.7 Analysis of cracked members A realistic analysis of concrete structures needs to account for the effects of cracking of the concrete. This is certainly important for calculations carried out at service conditions where signiﬁcant errors in the evaluation of deformations and stresses will arise if the effects of cracking are not included. In Chapter 7, cracking of the concrete is included in the cross-sectional analysis in one of two ways. In the ﬁrst more approximate approach, the extent of cracking is determined from the instantaneous analysis assuming the concrete can carry no tension and, for the time analysis, the extent of cracking and the depth of the intact concrete on the cross-section are assumed to remain unchanged. The second approach to the time analysis of a cracked cross-section is a more reﬁned method of analysis that traces the crack development with time by accounting for the change in the depth of the concrete compressive zone as time progresses. This latter approach is particularly suitable for the analysis and design of structural members where deﬂection or crack control at the serviceability limit states are the governing design considerations. In the following, the application of these two approaches using the stiffness method and the ﬁnite-element approach is discussed. More advanced non-linear software for modelling cracking in concrete structures is available, but the two proposed methods provide a practical balance between the complexity adopted in the analysis and the variability of the concrete properties required for input into the analysis. 9.7.1 Approach 1 Cracking occurs when the stresses in the concrete produced by applied loads or deformations reach the tensile strength of the concrete. In the case of statically indeterminate members, the internal actions at a particular cross-section depend on the extent of cracking and this is usually unknown at the beginning of the analysis. A simple and practical method for including cracking in the analysis of a structure involves an iterative procedure that is illustrated here by considering the propped cantilever shown in Fig. 9.11. The ﬁrst iteration involves the analysis of the structure using either the stiffness or ﬁnite-element methods assuming the whole structure to be uncracked (Fig. 9.11b) following the procedures presented in the previous sections. Based on these results, the extent of cracking to be used in the second iteration is determined. In the propped cantilever of Fig. 9.11c, cracking occurs in that part of the beam adjacent to the ﬁxed support where the applied moment is greater than the cracking moment Mcr (where Mcr was introduced in Chapter 3 and is the moment required to produce an extreme ﬁbre tensile stress in the concrete equal to its tensile strength). The cross-sectional properties of the cracked region are next obtained following the procedure presented in Chapter 7 and the member is then re-analysed using the revised cross-sectional rigidities. At the end of the second iteration, the lengths of the cracked and uncracked segments are adjusted based on the revised bending moment diagram, as shown in Fig. 9.11d, and the updated stiffnesses are adopted for the third iteration. The adjustments of the cracked and uncracked lengths continue until two subsequent iterations produce negligible differences. The implementation of the convergence criteria can be carried out in different ways depending on the modelling technique adopted. For example, the beam shown in

388 Stiffness method and ﬁnite-element modelling

(a) Support and loading arrangements.

Uncracked (b) Iteration 1: Uncracked length and bending moment diagram. Mcr Mcr

M

Cracked

Uncracked

(c) Iteration 2: Cracked and uncracked segments and bending moment diagram Mcr Mcr M Cracked Uncracked

Cracked Uncracked

(d) Iteration 3: Cracked and uncracked segments and bending moment diagram.

Mcr Mcr M

Figure 9.11 First iterations of the analysis of a propped cantilever using approach 1.

Fig. 9.11 could be modelled using different stiffness (or ﬁnite) elements for each cracked and uncracked region. The lengths of the cracked and uncracked segments would change from iteration to iteration. Convergence is achieved when the required adjustments of lengths for each segment is negligible. This approach can be applied only for simple members, such as the one shown in Fig. 9.11, as its use becomes prohibitive for large systems. In the case of more complex structures, it is preferable to discretise the whole structure using a predeﬁned element mesh and to assign to each element either cracked or uncracked properties based on the calculated internal actions. In this case, the ﬁrst iteration is also carried out assuming all elements are uncracked. After the instantaneous solution at time τ0 is completed, the time analysis is carried out assuming

Stiffness method and ﬁnite-element modelling 389 the extent of the cracked and uncracked regions does not change with time. For this purpose, the use of the AEMM to determine the time-dependent behaviour is recommended. In this way, only one additional analysis is required with no further iterations. Clearly, the method does not account for time-dependent cracking, as no attempt is made to discretise the time domain. This method is suitable for modelling structures when only linear-elastic analysis software is available. 9.7.2 Approach 2 The main advantage of this second approach relies on its ability to follow the occurrence and development of cracking throughout the structure. This is particularly useful for structural elements recognised to be critical at service conditions. In the more reﬁned, second approach, the structure is discretised into a predetermined layout of elements, with the number and size of elements selected depending on the degree of accuracy required. The extent of initial cracking in the structure is then determined by performing a non-linear analysis at time τ0 . This is usually based on well-known non-linear solution strategies such as the secant or Newthon–Raphson methods. Both can be implemented with the stiffness and ﬁnite element methods, even if the latter is naturally more suitable for these types of analysis. In fact, when using the ﬁnite element approach to analyse a concrete structure, the non-linear response of the concrete is accounted for in the numerical integration of the stiffness coefﬁcients and of the load vectors. Considering the line element shown in Fig. 9.6, these approximations are applied to the integrals of Eqs A.25 and A.26 following procedures well established for the ﬁnite element method (Refs 2 and 4). In this process, the section is subdivided into smaller areas in order to better depict the non-linear response, such as the layered cross-sections already discussed in Section 7.4. With the stiffness method, the appropriate cross-sectional rigidities are calculated at one or more locations along the member length following the approach presented in Chapter 7. When the instantaneous analysis is completed, the time analysis is carried out by discretising the time domain into a number of steps and modelling the concrete behaviour using the SSM. With this approach, the time-dependent behaviour of the concrete is carefully monitored at the integration points along each element. The main non-linearity addressed in this analysis originates from the fact that the concrete is assumed not to be able to carry tensile stresses greater than its tensile strength. If at any time instant the concrete stress at any calculation point exceeds the tensile strength, the previously stored stress history at this point is set to zero, the contribution to element stiffness is adjusted and the structure is reanalysed. The process continues until no new cracking is identiﬁed at any point in the structure. Of course, if a cracked point is later subjected to compressive stresses during subsequent time steps, the point again becomes active and contributes to the element stiffness. Obviously, tension-stiffening could also be included in the analysis, even if its time-dependent behaviour is still the focus of current research (Ref. 6).

9.8 References 1. Hibbeler, R.C. (2009). Structural Analysis. Seventh edition, Pearson Prentice Hall. 2. Bathe, K.J. (2006). Finite Element Procedures. Prentice Hall, New Jersey.

390 Stiffness method and ﬁnite-element modelling 3. Weaver, W. and Gere, J.M. (1990). Matrix Analysis of Framed Structures. Third edition, Van Nostrand Reinhold, New York. 4. CEB-FIB (2008). Practitioners’ Guide to Finite Element Modelling of Reinforced Concrete Structures. International Federation for Structural Concrete, ﬁb Bulletin 45, Lausanne, Switzerland. 5. Crisﬁeld, M.A. (1991). The eccentricity issue in the design of plate and shell elements. Communications in Applied Numerical Methods, 7, 47–56. 6. Gilbert, R.I. and Wu, H.Q. (2009). Time-dependent stiffness of cracked reinforced concrete elements under sustained actions. Australian Journal of Structural Engineering, Engineers Australia, 9(2) 151–158. 7. Gupta, A.K. and Ma, P.S. (1977). Error in eccentric beam formulation. International Journal for Numerical Methods in Engineering, 11, 1473–1483. 8. Ranzi, G. and Zona, A. (2007). A composite beam model including the shear deformability of the steel component. Engineering Structures, 29, 3026–3041.

Appendix A Analytical formulations Euler–Bernoulli beam model

A.1 Introduction The Euler–Bernoulli beam model is widely used for the analysis of structures. Designers use it on a daily basis in the form of either closed form solutions, such as those provided for the estimate of elastic deﬂections, or line (frame) elements for the prediction of deformations and internal actions using commercial structural analysis software. The analytical formulation at the basis of the Euler–Bernoulli beam model is described in the following sections for generic concrete members (such as those shown in Fig. A.1), where a perfect bond is assumed between the concrete and the reinforcement. The weak form of the model (global balance condition) is presented to provide a basis for the ﬁnite element formulation brieﬂy introduced in Chapter 9. The strong form (local balance condition) is then obtained by integrating this by parts. This has been used to derive the stiffness matrix and equivalent nodal actions required for the stiffness method described in Chapter 9. The proposed formulations are derived for a typical instant in time and, because of this, could be applicable to both short- and long-term analyses. For ease of notation, additional subscripts are included in this appendix to identify the time step under

z

L x y

(a) Reinforced concrete beam

z

L x y

(b) Prestressed concrete beam

Figure A.1 Typical concrete members and cross-sections.

392 Analytical formulations consideration only when it may not be clear from the context. A similar approach is used when deﬁning the time dependency of variables. For example, the deﬂection along the member length that is a function of both member coordinate z and time t will be referred to as v(z) (or simply v) instead of v(t, z).

A.2 Kinematic model In the undeformed state, the beam is assumed to be prismatic with the ortho-normal reference axis system {O; x, y, z} as shown in Fig. A.1. The kinematic behaviour is illustrated in Fig. A.2b for a generic point P on the z-axis, highlighting both its axial displacement at the level of the reference axis u(z) and its deﬂection v(z). The formulation is derived for a beam segment of length L and the cross-section is assumed to be symmetric about the y-axis. Under these assumptions, no torsional and out-of-plane ﬂexural effects are considered. The level of the reference x-axis is arbitrary. Considering a point Q located away from the member axis, its ﬁnal displacement can be expressed in terms of u(z) and v(z) as well as the rotation θ(z). In particular, the vertical and horizontal displacements, referred to as dy (y, z) and dz (y, z), can be expressed as: dy (y, z) = v (z) − y + y cos θ (z)

(A.1a)

dz (y, z) = u (z) − y sin θ (z)

(A.1b)

and, for clarity, the kinematic response of the point Q is illustrated in Fig. A.2c. The expressions of Eqs A.1 describe all possible displacements that the points of the beam can undergo. This set of displacements is usually referred to as the displacement ﬁeld of the model. For structural engineering applications, it is usually sufﬁcient and z

P L Elevation

y

Section

(a ) P

u(z)

P

z yQ

v(z)

z dz(y, z)

Q

y

y dy(y, z)

(b)

P′

q(z)

q(z)

(c)

P′

yQcos(q(z)) yQsin(q(z))

Figure A.2 Displacement ﬁeld.

Q′

Analytical formulations 393 convenient to remain within the framework of small displacements. In this way, the cosine and sine of the angle θ(z) in Eqs A.1 can be approximated by: cos θ(z) ≈ 1 and sin θ(z) ≈ θ(z). Consistent with the assumptions of the Euler-Bernoulli beam model, plane sections are assumed to remain plane and perpendicular to the beam axis before and after deformations. This condition implies that: θ (z) = v (z)

(A.2)

where the prime represents differentiation with respect to z. Based on these simpliﬁcations the displacement ﬁeld of Eqs A.1 can be re-written as: dy (y, z) = v (z)

(A.3a)

dz (y, z) = u (z) − y θ (z) = u (z) − yv (z)

(A.3b)

Equations A.3 show how the kinematic response of a point in the beam can be determined when the displacements u(z) and v(z) are known. For ease of notation, u(z), v(z) and θ(z) will be referred to as u, v and θ, respectively, in the following. Based on the adopted displacement ﬁeld, the only non zero strain is: εz = u − yv

(A.4)

where εz is the axial strain of the member. The expression for the curvature κ(= −v ) can be obtained by differentiating the deﬂection v twice with respect to the coordinate z, and the negative sign in front of v is required in ﬂexural members to produce a positive curvature in sagging moment regions (i.e. where compressive and tensile strains occur in the top and bottom ﬁbres of the section in a horizontal beam, respectively, in accordance with the sign convention adopted in this book).

A.3 Weak formulation (global balance condition) The weak form of the structural formulation for the frame element is obtained using the principle of virtual work considering a beam segment of length L with the free body diagram shown in Fig. A.3. In particular, p(z) and n(z) represent the vertical and horizontal distributed member loads which, for ease of notation, will be referred to as p and n in the following. The nodal actions at each end of the member represent external loads or reactions depending on the boundary conditions of the beam segment and have been referred to as S, N and M with the subscripts L and R specifying whether they relate to the left (at z = 0) or right (at z = L) ends of the member, respectively, as shown in Fig. A.3. The derivation is carried out by equating the work of internal stresses to the work of external actions for each virtual admissible variation of the displacements and corresponding strains (which, by deﬁnition, represent all variations of

394 Analytical formulations p(z) MR

ML NL

NR

n(z) SL

SR

z L

Figure A.3 Member loads and nodal actions.

possible displacements satisfying the kinematic boundary conditions of the problem) as follows: σz εˆ z dA dz = pˆv +nuˆ dz +SL vˆ L +NL uˆ L +ML θˆL +SR vˆ R +NR uˆ R +MR θˆR L A

L

(A.5)

where the variables with the hat ‘ˆ’ represent virtual variations of displacements or strains. Substituting the expression for the axial strain εz of Eq. A.4 into Eq. A.5, the weak form of the derivation can be re-written as: pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL σz uˆ − yˆv dA dz = L A

L

+ SR vˆ R + NR uˆ R + MR θˆR

(A.6)

Recalling the deﬁnitions of internal axial force N and moment M (about the x-axis) introduced in Chapter 5 and reproduced here for ease of reference: Ni =

A

σz dA

and

Mi =

A

yσz dA

(A.7a,b)

the integral at the cross-section (i.e. in dA) present on the left-hand side of Eq. A.6 can be replaced by these internal actions as: L

Ni uˆ − Mi vˆ dz =

L

pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL

+ SR vˆ R + NR uˆ R + MR θˆR

(A.8)

This relationship can be further rearranged to isolate the terms related to Ni and Mi as follows: ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ ⎤ ⎡ vˆ L SR vˆ R SL Ni uˆ n uˆ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ · dz = · dz + ⎣ NL ⎦ · ⎣uˆ L ⎦ + ⎣ NR ⎦ · ⎣uˆ R ⎦ Mi −ˆv vˆ L p ML θˆL MR θˆR

L

(A.9)

Analytical formulations 395 It is possible to ignore the nodal actions included on the right-hand side of Eq. A.9 as these can be easily included in the frame analysis during the assembly of the load vector. Based on this, Eq. A.9 can be simpliﬁed to: L

Ni uˆ n uˆ · dz = · dz Mi −ˆv vˆ L p

(A.10)

In this form, the constitutive models for the materials are not explicitly speciﬁed as they are included in the deﬁnitions of the internal actions Ni and Mi . To remain consistent with the notation adopted in the rest of the book, the expressions already introduced in Chapter 5 (reproduced here for ease of reference) are adopted in the following to deﬁne the internal actions as a function of the material properties: ri = Dε + fcr − fsh

(A.11)

which can be written highlighting the terms included in the matrix and vectors as: RA Ni = Mi RB

RB RI

εr κ

+

fcrN

fcrM

−

fshN

(A.12)

fshM

and the cross-sectional rigidities RA , RB and RI are deﬁned in Chapter 5 for different types of cross-sections. In particular, ri collects the internal axial force Ni and internal moment Mi , D speciﬁes the geometric and material properties of the cross-section, ε includes the strain calculated at the level of the reference axis εr and the curvature κ which can be expressed in terms of the horizontal and vertical displacements (i.e. u and v) as shown below, while f cr and f sh account for creep and shrinkage effects, respectively: 1 Ni σz dA RA A = 1 ; D= ri = Mi yσ dA RB z A f f fcr = crN and fsh = shN fcrM fshM

RB RI

;

ε=

εr κ

u = −v

(A.13a,b,c)

(A.13d,e)

This representation of f cr and f sh is particularly useful as it enables the proposed derivation to be applicable when using either the age-adjusted effective modulus method (AEMM) or the step-by-step method (SSM). When using the AEMM the components of f cr and f sh are determined as: fcrN =

Ac

fcrM =

Ac

Fe,0 σc,0 dA = Fe,0 Nc,0 Fe,0 yσc,0 dA = Fe,0 Mc,0

and fshN = Ee,k Ac εsh,k and fshM = Ee,k Bc εsh,k

(A.14a,b) (A.14c,d)

396 Analytical formulations where Ee,k and Fe,0 are deﬁned in Eqs 4.35 and 4.46. When using the SSM, these components at time τk become: fcrN =

fcrM =

k−1 i=0 Ac k−1 i=0 Ac

k−1

Fe,k,i σc,i dA =

Fe,k,i Nc,i and fshN = Ec,k Ac εsh,k

(A.15a,b)

i=0

Fe,k,i yσc,i dA =

k−1

Fe,k,i Mc,i and fshM = Ec,k Bc εsh,k

(A.15c,d)

i=0

where σc,i is the stress in the concrete at time τi , while Nc,i and Mc,i represent the axial force and moment, respectively, resisted by the concrete component at time τi . The vector ε can also be re-written in terms of the independent displacements u and v as: ε=

εr κ

u ∂ 0 u = = = Ae 2 −v 0 −∂ v

(A.16)

where A is a differential operator and the symbol ∂ deﬁnes the derivative with respect to the member coordinate z and the displacements u and v are collected in vector e as: u e= v

(A.17)

At this point it is useful to re-write Eq. A.10 in terms of vectors ri and ε (= A e): L

ri · A eˆ dz =

L

q · eˆ dz

(A.18)

where the member loads n and p have been collected in the vector q as: q=

n

(A.19a,b)

p

Substituting the constitutive properties deﬁned in Eq. A.11 into Eq. A.18 produces the general expression for the weak form accounting for time effects: L

Dε + fcr − fsh · A eˆ dz =

L

q · eˆ dz

(A.20)

A.4 Finite element formulation The formulation proposed in the following is applicable to displacement-based ﬁnite elements. If necessary, the approach can be extended to other elements, i.e. forcebased or mixed elements. The basis of the ﬁnite element formulation relies on the

Analytical formulations 397 approximation of the independent displacements u and v, previously collected in the vector e. This approximation can be expressed as: e∼ = N e de

(A.21)

in which Ne is the matrix that speciﬁes the adopted shape functions and de is the vector of the nodal displacements of the ﬁnite element. Substituting the approximation of Eq. A.21 into Eq. A.20 produces the weak form of the problem expressed in terms of nodal displacements: L

Dε + fcr − fsh · A Ne dˆ e dz =

L

q · Ne dˆ e dz

(A.22)

This relationship can be re-arranged to isolate the virtual nodal displacements dˆ e on one side of the dot product: L

(A Ne )T Dε + fcr − fsh dz · dˆ e =

L

NeT q dz · dˆ e

(A.23)

from which the stiffness relationship of the ﬁnite element can be obtained: ke de = pe

(A.24)

where ke is the ﬁnite element stiffness matrix and pe represents the loading vector related to both member loads and time effects. In particular, these are deﬁned as: ke =

L

(A Ne )T D ε dz =

L

(A Ne )T D (A Ne ) dz

(A.25a)

pe = pe.m − pe.cr + pe.sh

(A.25b)

where the loading vector pe has been separated into pe.m , pe.cr , and pe.sh relating to member loads (n and p), creep effects and shrinkage effects, respectively, and given by: pe.m =

L

NeT q

dz;

pe.cr =

T

L

(A Ne ) fcr dz;

and pe.sh =

L

(A Ne )T fsh dz (A.26a–c)

Conventional ﬁnite element procedures are then utilized to assemble the vectors and matrices for the whole structure and to perform the structural analysis (Refs 1 and 2). The derivations are outlined in the following by means of worked examples. A.4.1 Age-adjusted effective modulus method Expressions for the stiffness matrix and loading vectors related to member loads, creep effects and shrinkage effects for the 7 DOF ﬁnite element shown in Fig. 9.6 are derived here. For this element, the axial (u) and transverse displacements (v) are approximated using parabolic and cubic functions, respectively. The time-dependent behaviour of the

398 Analytical formulations concrete is modelled using the AEMM speciﬁed in Eq. 4.45 (Approach 2 in Section 4.4.4). The parabolic and cubic approximation for the axial and vertical displacements of the 7 dof element are: u = Nu1 uL + Nu2 uM + Nu3 uR

and v = Nv1 vL + Nv2 θL + Nv3 vR + Nv4 θR (A.27a,b)

where: Nu1 = 1 −

3z 2z2 + 2; L L

Nv1 = 1 −

3z2 2z3 + 3; L2 L

3z2 2z3 − 3; L2 L

Nv3 =

Nu2 =

4z 4z2 − 2; L L

Nv2 = z −

Nv4 = −

Nu3 = −

z 2z2 + 2 L L

(A.28a–c)

2z2 z3 + 2; L L

(A.29a,b)

z2 z3 + L L2

(A.29c,d)

It is usually convenient to represent these approximations by means of the matrix of shape functions Ne and a vector de collecting the nodal displacements: ⎤ uL ⎢ ⎥ ⎢ vL ⎥ ⎢ ⎥ ⎢ θ ⎥ ⎢ L⎥ 0 ⎢ ⎥ ⎢uM ⎥ = Ne de ⎥ Nv4 ⎢ ⎢u ⎥ ⎢ R⎥ ⎢ ⎥ ⎣ vR ⎦ ⎡

u v

=

Nu1 0

0

0

Nu2

Nu3

0

Nv1

Nv2

0

0

Nv3

(A.30)

θR The stiffness matrix of the 7 DOF ﬁnite element can be calculated based on Eq. A.25a. This requires the calculation of A Ne which, recalling the deﬁnition of the differential operator A speciﬁed in Eq. A.16, is obtained as: ⎡

A Ne

N = ⎣ u1 0

⎡

0

0

−Nv1

−Nv2

⎢− 3 + 4z ⎢ L L2 =⎢ ⎢ ⎣ 0

Nu2

0

⎤

Nu3

0

0

−Nv3

0

0

12z 6 − 3 L2 L

4 6z − L L2

0 ⎦ −Nv4

⎤

4 8z 1 4z − + 2 − L L2 L L 0

0

0 −

6 12z + 3 L2 L

0

⎥ ⎥ ⎥ ⎥ 6z ⎦

2 − L L2

Analytical formulations 399 Substituting the expression obtained for A Ne into Eq. A.25a and carrying out the integration along the member length produces the element stiffness matrix: ⎡ ⎢ 7RA ⎢ 3L ⎢ ⎢ ⎢ −4RB ⎢ ⎢ L2 ⎢ ⎢ ⎢ −3RB ⎢ ⎢ ⎢ L ⎢ ⎢ ke = ⎢ −8RA ⎢ ⎢ 3L ⎢ ⎢ R ⎢ A ⎢ ⎢ 3L ⎢ ⎢ ⎢ 4RB ⎢ ⎢ L2 ⎢ ⎣ −RB L

−4RB L2

−3RB L

−8RA 3L

RA 3L

4RB L2

12RI L3

6RI L2

8RB L2

−4RB L2

−12RI L3

6RI L2

4RI L

4RB L

−RB L

−6RI L2

8RB L2

4RB L

16RA 3L

−8RA 3L

−8RB L2

−4RB L2

−RB L

−8RA 3L

7RA 3L

4RB L2

−12RI L3

−6RI L2

−8RB L2

4RB L2

12RI L3

6RI L2

2RI L

4RB L

−3RB L

−6RI L2

⎤ −RB ⎥ L ⎥ ⎥ ⎥ 6RI ⎥ ⎥ L2 ⎥ ⎥ ⎥ 2RI ⎥ ⎥ ⎥ L ⎥ ⎥ 4RB ⎥ ⎥ ⎥ L ⎥ ⎥ −3RB ⎥ ⎥ ⎥ L ⎥ ⎥ ⎥ −6RI ⎥ ⎥ L2 ⎥ ⎥ ⎦ 4RI L

(A.31)

Recalling the expression previously obtained for A Ne , the loading vectors are then calculated based on Eqs A.26. In particular, the one related to the member loads n and p can be derived as: ⎡

⎡ Nu1 ⎢ ⎢ 0 ⎢ ⎢ ⎢ 0 ⎢ pe.m = NeT q dz = ⎢ ⎢Nu2 L L⎢ ⎢Nu3 ⎢ ⎢ ⎣ 0 0

⎤ L ⎢ ⎥ ⎢ 6n ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ L ⎥ ⎢ ⎤ p ⎥ ⎢ ⎥ 2 ⎢ ⎥ 0 ⎢ ⎥ ⎥ ⎢ ⎥ 2 L Nv1 ⎥ ⎢ ⎥ ⎥ p ⎢ ⎥ ⎥ 12 ⎢ ⎥ Nv2 ⎥ ⎢ ⎥ ⎥ n ⎢ ⎥ ⎥ 2L dz = ⎢ ⎥ 0 ⎥ n ⎢ ⎥ p ⎥ ⎢ ⎥ 3 0 ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎥ L ⎢ ⎥ Nv3 ⎦ n ⎥ ⎢ ⎢ 6 ⎥ ⎢ ⎥ Nv4 ⎢ ⎥ ⎢ L ⎥ ⎢ p ⎥ ⎢ 2 ⎥ ⎢ ⎥ ⎣ ⎦ L2 − p 12

(A.32)

As highlighted in Eq. A.26b, the calculation of the loading vector describing creep effects pe.cr requires the knowledge of the axial force and moment for the calculation of fcrN and fcrM included in f cr . These depend to the loading history of the concrete as

400 Analytical formulations both fcrN and fcrM are determined by multiplying the axial force and moment resisted by the concrete at one or more instants in time by particular material coefﬁcients. The deﬁnition of these coefﬁcients varies depending on the constitutive relationship for concrete and, for the AEMM, it is given in Eqs A.14. The analysis at a particular instant in time can be carried out only if the instantaneous analysis has been completed and the concrete stress resultants recorded. The actual recording of these actions can be carried out by storing the values of the concrete axial force and moment at particular locations along each member. These locations are usually those required by the numerical integration of Eq. A.26b. Another option is to identify polynomials capable of describing the variation of the concrete axial force and moment along each element and to store the relevant coefﬁcients. This option is preferred here as it enables closed form solutions to be obtained. The orders of the polynomial describing fcrN and fcrM (Eqs A.14) depend on the orders of the expressions for the axial force and moment resisted by the concrete at time τ0 , Nc.0 and Mc.0 . Recalling that: σc,0 dA = Ec,0 u0 − yv0 dA = Ac Ec,0 u0 − Bc Ec,0 v0 (A.33a) Nc,0 = Ac

Ac

Mc,0 =

Ac

yσc,0 dA =

Ac

yEc,0 u0 − yv0 dA = Bc Ec,0 u0 − Ic Ec,0 v0

(A.33b)

and considering that, in the 7 DOF ﬁnite element (Fig. 9.6), u and v are approximated by a parabolic and a cubic polynomial, respectively, the actual functions describing Nc,0 and Mc,0 determined using Eqs A.33 become linear and can be expressed as: Nc.0 = ac0,0 + ac1,0 z

and Mc.0 = bc0,0 + bc1,0 z

where the coefﬁcients ac0,0 , ac1,0 , bc0,0 , and bc1,0 are determined from Eqs A.33. Considering Eqs A.27–A.30, the expressions for u0 and v0 can be written in terms of the nodal displacements of the ﬁnite element as: uL,0 +Nu2 uM,0 +Nu3 uR,0 u0 = Nu1

3 4z 4 8z 1 4z = − + 2 uL,0 + uM,0 + − + 2 uR,0 − L L L L2 L L

3 4 1 4 8 4 = − uL,0 + uM,0 − uR,0 + uL,0 − 2 uM,0 + 2 uR,0 z L L L L2 L L

(A.34a)

v0 = Nv1 vL,0 +Nv2 θL,0 +Nv3 vR,0 +Nv4 θR,0

6 12z 4 6z 6 12z 2 6z = − 2 + 3 vL,0 + − + 2 θL,0 + − v + − θR,0 + R,0 L L L L2 L L L2 L 3

6 4 6 2 12 6 12 6 = − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 + 3 vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z L L L L L L L L (A.34b)

The ‘0’ subscript in the nodal freedoms in Eqs A34 is to specify that these are calculated at time τ0 .

Analytical formulations 401 The expression for the concrete axial force Nc,0 can then be obtained by substituting Eqs A.34 into Eq. A.33a:

Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0

3 4 1 4 8 4 = Ac Ec,0 − uL,0 + uM,0 − uR,0 + u − u + u L,0 M,0 R,0 z L L L L2 L2 L2

6 4 6 2 − Bc Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

12 6 12 6 + vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z 3 L L L L = ac0,0 + ac1,0 z

(A.35a)

where:

3 4 1 ac0,0 = Ac Ec,0 − uL,0 + uM,0 − uR,0 L L L

6 4 6 2 − Bc Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

4 8 4 ac1,0 = Ac Ec,0 uL,0 − 2 uM,0 + 2 uR,0 L2 L L

12 6 12 6 − Bc Ec,0 v + θ − v + θ L,0 L,0 R,0 R,0 L3 L2 L3 L2

(A.35b)

(A.35c)

Similarly, substituting Eqs A.34 into Eq. A.33b leads to the expression for Mc,0 :

Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0

3 4 1 4 8 4 = Bc Ec,0 − uL,0 + uM,0 − uR,0 + z u − u + u L,0 M,0 R,0 L L L L2 L2 L2

6 4 6 2 − Ic Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

12 6 12 6 + vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 z L3 L L L = bc0,0 + bc1,0 z

(A.35d)

402 Analytical formulations where:

3 4 1 bc0,0 = Bc Ec,0 − uL,0 + uM,0 − uR,0 L L L

6 4 6 2 − Ic Ec,0 − 2 vL,0 − θL,0 + 2 vR,0 − θR,0 L L L L

4 8 4 bc1,0 = Bc Ec,0 uL,0 − 2 uM,0 + 2 uR,0 2 L L L

12 6 12 6 − Ic Ec,0 vL,0 + 2 θL,0 − 3 vR,0 + 2 θR,0 L3 L L L

(A.35e)

(A.35f)

At this point, it is possible to derive the expressions for fcrN and fcrM substituting Eqs A.35 into Eqs A.14a and c: Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z fcrN = fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z and pe.cr can then be obtained as follows: pe.cr = (A Ne )T fcr dz L

⎡

⎤

⎢− 3 + 4z2 ⎢ L L

⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ = ⎢ 4 − 8z L⎢ ⎢ L L2 ⎢ 1 4z ⎢− + ⎢ L L2 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎣ 0

⎥ ⎥ ⎡ ⎤ ⎥ L −ac0,0 − ac1,0 12z ⎥ 6 6 − 3 ⎥ ⎢ ⎥ L2 L ⎥ ⎢ ⎥ ⎥ −b c1,0 ⎢ ⎥ ⎢ ⎥ 4 6z ⎥ − 2 ⎥ ⎢ ⎥ b c0,0 L L ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ F a + a z ⎥ e,0 c0,0 2 c1,0 ⎢ dz = Fe,0 ⎢ − Lac1,0 ⎥ ⎥ ⎥ 0 ⎥ 3 ⎢ ⎥ ⎥ Fe,0 bc0,0 + bc1,0 z 5 ⎢ ⎥ ⎥ La + a ⎢ ⎥ c1,0 c0,0 ⎥ ⎢6 ⎥ 0 ⎥ ⎢ ⎥ ⎥ ⎣ ⎦ bc1,0 ⎥ 12z ⎥ 6 − 2+ 3 ⎥ −bc1,0 L − bc0,0 L L ⎥ ⎦ 0

2 6z − L L2

(A.36)

The loading vector describing shrinkage effects pe.sh can be determined based on Eq. A.26c. If shrinkage does not vary along a member, fshN and fshM required to deﬁne f sh in Eq. A.26c are constant and for the AEMM are given by: Ee,k εsh,k dA = Ee,k Ac εsh,k and fshM = y Ee,k εsh,k dA = Ee,k Bc εsh,k fshN = Ac

Ac

The assumption of uniform shrinkage is usually acceptable for most practical applications.

Analytical formulations 403 The shrinkage loading vector pe.sh can then be calculated as: pe.sh = (A Ne )T fsh dz L

⎡

⎤

3 4z ⎢− + 2 ⎢ L L

⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ × ⎢ 4 − 8z 2 L⎢ ⎢ L L ⎢ 1 4z ⎢− + ⎢ L L2 ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎣ 0

⎤ ⎡ ⎥ ⎥ Ee,k Ac εsh,k ⎥ ⎥ ⎢ − ⎥ ⎢ 6 12z ⎥ ⎥ ⎥ ⎢ − 2 3 ⎥ ⎥ ⎢ 0 L L ⎥ ⎥ ⎢ ⎥ ⎢ 4 6z Ee,k Bc εsh,k ⎥ ⎥⎡ ⎥ ⎢ − ⎤ ⎥ ⎢ L L2 ⎥ L ⎥ ⎥ ⎢ ⎥ ⎣Ee,k Ac εsh,k ⎦ ⎥ ⎢ dz = ⎢ ⎥ ⎥ 0 0 ⎥ ⎥ ⎢ ⎥ Ee,k Bc εsh,k ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎢ Ee,k Ac εsh,k ⎥ 0 ⎥ ⎥ ⎢ ⎥ ⎥ ⎢ ⎥ ⎥ ⎢ 6 12z ⎥ 0 ⎥ ⎢ − + ⎥ ⎦ ⎣ L2 L3 ⎥ Ee,k Bc εsh,k ⎦ − 2 6z 0

L

−

L2

(A.37)

L

A.4.2 Step-by-step method The 7 DOF ﬁnite element of the previous section is reconsidered here with the timedependent behaviour of the concrete described using the SSM. The change in the representation of the concrete time-dependent behaviour only affects the calculation of the loading vectors accounting for creep and shrinkage effects. In fact, the stiffness matrix and the vectors depicting member loads and shrinkage are always deﬁned using the cross-sectional properties relevant to the time step under consideration. In particular, with the SSM the concrete contributions are determined using Ec,k introduced in Eqs 4.25 and 4.26. Similarly to the AEMM, the loading vector describing creep effects pe.cr can be determined once the values of fcrN and fcrM included in f cr are determined. The expressions of these terms calculated using the SSM are deﬁned in Eqs A.15a and c. Also in this case, polynomials are utilized to represent the variation of the concrete axial force and moment along the element length measured at different time steps. For this purpose, the coefﬁcients included in these polynomials need to be recorded at each instant in time. Another possible approach would rely on the use of a numerical integration for the calculation of fcrN,k and fcrM,k . In this case, the concrete axial force and moment obtained at particular locations along each element (and required for the numerical integration) need to be stored. As the orders of the functions representing the concrete axial force and moment do not vary with time, the polynomials already identiﬁed for the AEMM in the previous example to describe the concrete instantaneous response are now adopted for each time instant. The concrete axial force and moment at time τi may be expressed as: Nc.i = ac0,i + ac1,i z

and Mc.i = bc0,i + bc1,i z

(A.38a,b)

and the coefﬁcients ac0,i , ac1,i , bc0,i , and bc1,i are determined as outlined in the following.

404 Analytical formulations Considering the constitutive relationship for concrete introduced in Eq. 4.25 (reproduced here for ease of reference): σc,i = Ec,i (εi − εsh ) +

k−1

Fe,k,n σc,n

n=0

the deﬁnitions of both axial force and moment resisted by the concrete component at any time τi can be expressed as: i−1 σc,i dA = Ec,i ui − yvi − Ec,i εsh,i + Fe,i,n σc,n d A Nc,i = Ac

Ac

n=0

= Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i + Mc,i =

Ac

yσc,i dA =

Ac

Fe,i,n Nc,n

(A.39a)

n=0

i−1 y Ec,i ui − yvi − Ec,i εsh,i + Fe,i,n σc,n d A

i−1

n=0

= Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n

(A.39b)

n=0

Considering Eqs A.27–A.30, the expressions for ui and vi required in Eqs A.39 are determined in terms of nodal displacements as:

3 4 1 4 8 4 ui = − uL,i + uM,i − uR,i + uL,i − 2 uM,i + 2 uR,i z (A.40a) L L L L2 L L

6 4 6 2 12 6 12 6 vi = − 2 vL,i − θL,i + 2 vR,i − θR,i + v + θ − v + θ L,i L,i R,i R,i z L L L L L3 L2 L3 L2 (A.40b) Substituting Eqs A.40 into Eq. A.39a produces the expression for Nc,i in terms of nodal displacements, shrinkage and previous loading history: Nc,i = Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i +

i−1

Fe,i,n Nc,n

n=0

3 4 1 4 8 4 = Ac Ec,i − uL,i + uM,i − uR,i + uL,i − 2 uM,i + 2 uR,i z L L L L2 L L

6 4 6 2 − Bc Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i L L L L

12 6 12 6 + v + θ − v + θ L,i L,i R,i R,i z L3 L2 L3 L2 − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n + ac1,n z

n=0

= ac0,i + ac1,i z

(A.41a)

Analytical formulations 405 where:

3 4 1 ac0,i = Ac Ec,i − uL,i + uM,i − uR,i L L L

6 4 6 2 − Bc Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i L L L L − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n

n=0

4 8 4 ac1,i = Ac Ec,i uL,i − 2 uM,i + 2 uR,i L2 L L

i−1 12 6 12 6 v + θ − v + θ + Fe,i,n ac1,n − Bc Ec,i L,i L,i R,i R,i L3 L2 L3 L2 n=0

Similarly, for Mc,i :

Mc,i = Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n = bc0,i + bc1,i z

(A.41b)

n=0

where:

3 4 1 bc0,i = Bc Ec,i − uL,i + uM,i − uR,i L L L

i−1 6 4 6 2 Fe,i,n bc0,n − Ic Ec,i − 2 vL,i − θL,i + 2 vR,i − θR,i − Bc Ec,i εsh,i + L L L L n=0

4 8 4 bc1,i = Bc Ec,i u − u + u L,i M,i R,i L2 L2 L2

i−1 12 6 12 6 + v + θ − v + θ Fe,i,n bc1,n − Ic Ec,i L,i L,i R,i R,i L3 L2 L3 L2 n=0

The expressions for fcrN,k and fcrM,k can then be re-written as:

fcrN,k =

k−1

Fe,k,i Nc,i =

i=0

fcrM,k =

k−1 i=0

k−1

Fe,k,i ac0,i + ac1,i z

i=0

Fe,k,i Mc,i =

k−1 i=0

Fe,k,i bc0,i + bc1,i z

406 Analytical formulations and the loading vector related to creep effects pe.cr is obtained from: pe.cr = (A Ne )T fcr dz L

⎡

⎤

⎢− 3 + 4z ⎥ 0 ⎢ L L2 ⎥ ⎢ ⎥ ⎢ ⎥ ⎡ ⎤ ⎢ 12z ⎥ 6 L ⎢ 0 ⎥ − −ac0,i − ac1,i ⎢ L2 L3 ⎥ 6 ⎢ ⎥ ⎢ ⎥⎡ ⎢ ⎥ ⎤ ⎢ ⎥ −b c1,i ⎢ ⎥ 4 6z ⎥ ⎢ 0 ⎢ ⎥ − 2 ⎥ k−1 ⎢ ⎢ ⎢ ⎥ ⎥ L L b c0,i ⎥ ⎢ Fe,k,i ac0,i + ac1,i z ⎥ ⎢ k−1 ⎢ ⎥ ⎢ ⎥⎢ ⎥ ⎢ ⎥ ⎥ ⎢ i=0 Fe,k,i ⎢ − 2 Lac1,i ⎥ = ⎢ ⎥ dz = ⎢ 4 − 8z ⎥ 0 ⎢ ⎥ ⎢ ⎥ L ⎢ L L2 ⎥ ⎣k−1 ⎢5 3 ⎥ i=0 ⎢ ⎥ F b + b z⎦ ⎢ ⎥ La + a c0,i c1,i e,k,i ⎢ ⎥ ⎢ 6 c1,i c0,i ⎥ ⎢ 1 4z ⎥ i=0 ⎢ ⎥ 0 ⎢− + 2 ⎥ ⎣ ⎦ bc1,i ⎢ L L ⎥ ⎢ ⎥ ⎢ ⎥ −bc1,i L − bc0,i 12z 6 ⎢ 0 − 2+ 3 ⎥ ⎢ ⎥ L L ⎢ ⎥ ⎣ ⎦ 0

6z 2 − L L2

(A.42)

The loading vector related to shrinkage effects pe.sh is obtained from Eq. A.37, except that Ec,k replaces Ee,k .

A.5 Strong formulation (local balance condition) The strong form of the problem, consisting of the governing system of differential equations and corresponding boundary conditions, is obtained by integrating by parts the weak form presented in Eq. A.8, as follows: L L L Ni uˆ 0 − Ni uˆ dz − Mi vˆ 0 + Mi vˆ 0 − Mi vˆ dz =

L

L

L

pˆv + nuˆ dz + SL vˆ L + NL uˆ L + ML θˆL + SR vˆ R + NR uˆ R + MR θˆR

(A.43)

Enforcing horizontal and vertical equilibrium, the system of differential equations obtained from Eq. A.43 can then be expressed as: Ni + n = 0

and

Mi + p = 0

(A.44a,b)

From Eq. A.43, the corresponding boundary conditions to be applied at the left and right ends of the beam segment (i.e. at z = 0 and L) are: (NiL + NL ) uˆ L = 0; MiL + SL vˆ L = 0;

(NiR − NR ) uˆ R = 0 MiR − SR vˆ R = 0

(A.45a,b)

(MiL − ML ) θˆL = 0;

(MiR + MR ) θˆR = 0

(A.45e,f)

(A.45c,d)

Analytical formulations 407 The differential equations and their boundary conditions can also be deﬁned in terms of the independent displacements u and v by recalling the expressions for Ni and Mi of Eq. A.12: Ni = RA u − RB v + fcrN − fshN

(A.46a)

Mi = RB u − RI v + fcrM − fshM

(A.46b)

where the rigidities RA , RB and RI are deﬁned in Chapter 5 for different types of cross-sections. Substituting Eqs A.46 into Eqs A.44 and A.45 the differential equations can be re-written as: RA u − RB v + fcrN − fshN +n = 0

RB u − RI v

(A.47a)

+ fcrM − fshM +p = 0

(A.47b)

and the boundary conditions at the left (L) and right (R) ends of the member become: RA uL − RB vL + fcrNL − fshNL + NL uˆ L = 0 RA uR − RB vR + fcrNR − fshNR − NR uˆ R = 0 RB uL − RI vL + fcrML − fshML + SL vˆ L = 0 RB uR − RI vR + fcrMR − fshMR − SR vˆ R = 0 RB uL − RI vL + fcrML − fshML − ML θˆL = 0 RB uR − RI vR + fcrMR − fshMR + MR θˆR = 0

(A.48a) (A.48b) (A.48c) (A.48d) (A.48e) (A.48f)

The system of differential equations (Eqs A.47) is solved in the following, initially for the instantaneous material properties (i.e. no time effects) and then for the time analysis using the AEMM and the SSM. A.5.1 Instantaneous analysis Ignoring creep and shrinkage effects (i.e. fcrN = 0, fcrM = 0, fshN = 0 and fshM = 0), the general expressions for u and v which satisfy Eqs A.47 can be written as: v = α1 p

z4 z3 z2 + C1 + C2 + C3 z + C4 24 6 2

(A.49a)

u = α2 p

z3 z2 + (α3 C1 + α4 n) + C5 z + C6 6 2

(A.49b)

while the following coefﬁcients are been introduced to simplify the notation: α0 = R1 RA − R2B ;

α1 =

RA ; α0

α2 =

RB ; α0

α3 =

RB ; RA

and α4 =

−1 RA (A.50a–e)

408 Analytical formulations The constants of integration Cj (with j = 1, . . . , 6) can be determined based on the boundary conditions (Eqs A.48). In the following these analytical solutions have been used to derive the stiffness matrix and loading vector to be used in the stiffness method outlined in Chapter 9. A.5.1.1 Stiffness matrix Consider the unloaded ﬁxed ended beam shown in Fig. A.4a. The beam is modelled using a single 6 DOF stiffness element similar to that shown in Fig. 9.1 (i.e. three freedoms at each end node). The freedom numbering for the beam is shown in Fig. A.4b. The direct stiffness method is used here to derive the coefﬁcients of the stiffness matrix. The direct stiffness method is a procedure which enables the determination of the stiffness coefﬁcients by enforcing a unit displacement along one freedom while all other freedoms are restrained. The actual stiffness coefﬁcients are then equal to the reactions of the ﬁxed-ended beam required to keep the displaced conﬁguration. For example, enforcing a unit displacement along freedom 3 (i.e. rotation at the left support in Fig. A.4b), the reactions of the ﬁxed-ended beam correspond to the coefﬁcients included in the third column of the stiffness matrix. This approach is useful only when there is an analytical or numerical solution available to calculate the sought end reactions shown in Fig. A.4c. In the following, this will be carried out using the analytical solutions presented in Eqs A.49 combined with the boundary conditions of Eqs A.48. In order to calculate the coefﬁcients of the ﬁrst column of the stiffness matrix, a unit displacement is enforced along freedom 1 (Fig. A.4b), which corresponds to the axial displacement of the left node. For clarity, this deformation is shown in Fig. A.5. Considering that both member ends are fully restrained by the ﬁxed support conditions, the constants of integration included in the general solutions for u and v presented in Eqs A.49 can be determined by enforcing the following kinematic conditions:

6

3

z

1

4

2

L (a) Support conditions

5 (b) Numbering of the freedoms

ML

MR NR

NL SL

SR

z L (c) Freebody diagram

Figure A.4 Unloaded, ﬁxed-ended beam.

Analytical formulations 409 0

0

1

0

0

0

Figure A.5 A unit displacement enforced along freedom 1.

u (z = 0) = 1; u (z = L) = 0; and θ (z = L) = 0.

v (z = 0) = 0;

v (z = L) = 0;

θ (z = 0) = 0;

The calculated constants of integration can then be written as: C1 = 0;

C2 = 0;

C3 = 0;

C4 = 0;

1 C5 = − ; and C6 = 1. L

Adopting the static boundary conditions of Eqs A.48, the reactions of the ﬁxedended beam can be determined by solving the following equations for the unknown nodal actions (which represent the desired reactions): RA uL − RB vL + NL = 0;

RA uR − RB vR − NR = 0

RB uL − RI vL + SL = 0;

RB uR − RI vR − SR = 0

RB uL − RI vL − ML = 0;

RB uR − RI vR + MR = 0

where the expressions related to creep and shrinkage have been omitted as not relevant to the calculations of the stiffness coefﬁcients. The reactions required to maintain this deformed conﬁguration (Fig. A.5) can be collected in the following vector: ⎤ ⎡ ⎡ ⎤ RA /L NL ⎥ ⎢ ⎢ ⎥ ⎢ SL ⎥ ⎢ 0 ⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ML ⎥ ⎢ RB /L ⎥ p1 = ⎢ ⎥=⎢ ⎥ ⎢ NR ⎥ ⎢−RA /L⎥ ⎥ ⎢ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎣ SR ⎦ ⎣ 0 ⎦ −RB /L MR which deﬁnes the ﬁrst column of the stiffness matrix (identiﬁed by the subscript ‘1’). Considering a unit displacement along freedom 2 (Fig. A.6), the boundary conditions necessary to determine the constants of integration are: u (z = 0) = 0;

u (z = L) = 0;

v (z = 0) = 1;

v (z = L) = 0;

θ (z = 0) = 0;

and θ (z = L) = 0. and these produce the following expressions: C1 =

12 ; L3

C2 = −

6 ; L2

C3 = 0;

C4 = 1;

C5 = −

6 RB ; and C6 = 0. L 2 RA

410 Analytical formulations 0 0

0

0

0 1

Figure A.6 A unit displacement enforced along freedom 2.

Based on these constants of integration, the analytical solution for this displaced conﬁguration is described by a cubic function for the deﬂection v and a parabolic one for the axial displacement u, therefore providing consistent contributions to the strain ﬁeld from both v and u. The reactions, which form the second column of the stiffness matrix, are determined using the static boundary conditions of Eqs A.48 as: ⎡

⎤

0

⎥ ⎢ ⎢ 12 RI RA − R2B ⎥ ⎥ ⎡ ⎢ ⎤ ⎥ ⎢ L3 RA 0 NL ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ SL ⎥ ⎢ 6 RI RA − R2B ⎥ ⎢ 12/α1 L3 ⎥ ⎥ ⎢ ⎥ ⎢− ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ RA ⎥ ⎢ −6/α1 L2 ⎥ ⎢ M L ⎥ ⎢ L2 p2 = ⎢ ⎥=⎢ ⎥=⎢ ⎥ ⎥ ⎢ ⎥ ⎢ NR ⎥ ⎢ 0 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎣ SR ⎦ ⎢ 12 RI RA − R2B ⎥ ⎣−12/α1 L3 ⎦ ⎥ ⎢− ⎥ ⎢ L3 MR −6/α1 L2 RA ⎥ ⎢ ⎥ ⎢ ⎣ 6 RI RA − R2 ⎦ B − 2 RA L ⎡

⎤

Considering the remaining freedoms one at the time, the coefﬁcients of the whole stiffness matrix are determined: ⎡ ⎢ RA ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎢ ⎢ RB ⎢− ⎢ ke = ⎢ L ⎢ ⎢ RA ⎢− ⎢ L ⎢ ⎢ ⎢ ⎢ 0 ⎢ ⎢ ⎢ ⎣ R B L

⎤ 0

RB − L

RA − L

12 α1 L3

6 α1 L2

0

−

12 α 1 L3

6 α1 L2

R2 4 + B α1 L R A L

RB L

−

6 α 1 L2

0

RB L

RA L

0

0

12 α1 L3

−

12 α1 L 3

6 α1 L2

−

6 α1 L2

R2 2 − B α1 L R A L

−

RB L

0

−

6 α 1 L2

RB L

⎥ ⎥ ⎥ ⎥ ⎥ 6 ⎥ ⎥ α1 L 2 ⎥ ⎥ 2 RB ⎥ 2 ⎥ ⎥ − α1 L R A L ⎥ ⎥ ⎥ ⎥ RB ⎥ − ⎥ L ⎥ ⎥ ⎥ 6 ⎥ − ⎥ 2 α1 L ⎥ ⎥ 2 RB ⎦ 4 + α1 L R A L

(A.51)

Analytical formulations 411 A.5.1.2 Equivalent nodal actions for member loads Consider the ﬁxed-ended beam of the previous section subjected to constant member loads n and p (Fig. A.7). Eqs A.49 are used here to determine the equivalent nodal loads required to be used in the stiffness method of analysis. Note that this set of actions corresponds to the opposite of the reactions of the ﬁxed ended beam illustrated in Fig. A.7. As both member ends are fully restrained, the kinematic boundary conditions are: u (z = 0) = 0;

u (z = L) = 0;

v (z = 0) = 0;

v (z = L) = 0;

θ (z = 0) = 0;

and θ (z = L) = 0 and the expressions for the constants of integration are: L L2 α1 p; C3 = 0; C4 = 0; C1 = − α1 p; C2 = 2 12 3α1 α3 − 2α2 2 L C5 = L p − α4 n; and C6 = 0. 12 2 The reactions are obtained by solving the static boundary conditions of Eqs A.48 (ignoring time effects): RA uL − RB vL + NL = 0;

RB uL − RI vL + SL = 0;

RB uL − RI vL − ML = 0

RA uR − RB vR − NR = 0;

RB uR − RI vR − SR = 0;

RB uR − RI vR + MR = 0

and are given by: ⎤ ⎡ ⎡ ⎤ ⎡ ⎤ 0 NL.m −L/2 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎢ α3 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L2 /12⎥ ⎢Lα3 /2⎥ pF.m = ⎢ ⎥=⎢ ⎥ p+⎢ ⎥n ⎢ NR.m ⎥ ⎢ 0 ⎥ ⎢ −L/2 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ ⎣ α3 ⎦ L2 /12 MR.m Lα3 /2

(A.52)

where pF.m represents the reactions of the ﬁxed-ended beam subjected to constant longitudinal and transverse distributed loads, i.e. n and p. The equivalent nodal loads are equal and opposite to the reactions of pF.m . p

p MR

ML n

n

NR

NL SL

z

SR

z

L

L

(a) Loading and support conditions

(b) Free body diagram

Figure A.7 Fixed-ended beam subjected to constant member loads.

412 Analytical formulations A.5.1.3 Post-processing of the instantaneous solution From the instantaneous analysis, the axial force and moment resisted by the concrete at time τ0 are obtained from Eq. A.33. The deﬂection v0 and axial deformation u0 at any point z along a member are: z4 z3 z2 4,0 + C1,0 + C2,0 + C3,0 z + C 24 6 2 2 z3 6,0 1,0 + α4,0 n z + C 5,0 z + C u0 = α2,0 p + α3,0 C 6 2 v0 = α1,0 p

(A.53a) (A.53b)

where the constants αi,0 (i = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τ0 . Using the nodal displacements at each end of the member, the constants of integration are given by: 1,0 = − α1,0 L p + 6 θR,0 + θL,0 − 12 vR,0 − vL,0 C 2 L2 L3 2 2,0 = α1,0 L p − 2 θR,0 + 2θL,0 + 6 vR,0 − vL,0 C 2 12 L L C3,0 = θL,0 ; C4,0 = vL,0

5,0 = 3α1,0 α3,0 − 2α2,0 L2 p − α4,0 L n − 3α3,0 θR,0 + θL,0 C 12 2 L uR,0 − uL,0 6α3,0 − vL,0 − vR,0 + L L2 C6,0 = uL,0

(A.54a) (A.54b) (A.54c,d)

(A.54e) (A.54f)

The expressions for u0 and v0 can then be obtained by differentiating Eqs A.53: u0 = α2,0 p

z2 1,0 + α4,0 n z + C 5,0 + α3,0 C 2

(A.55a)

v0 = α1,0 p

z2 2,0 + C1,0 z + C 2

(A.55b)

The internal actions resisted by the concrete component can then be re-written as: Nc,0 = Ac Ec,0 u0 − Bc Ec,0 v0 z2 1,0 + α4,0 n z + C 5,0 = Ac Ec,0 α2,0 p + α3,0 C 2 z2 2,0 − Bc Ec,0 α1,0 p + C1,0 z + C 2 = ac0,0 + ac1,0 z + ac2,0 z2

(A.56)

Analytical formulations 413 where: 5,0 −Bc Ec,0 C 2,0 , ac0,0 = Ac Ec,0 C

1,0 +Ac Ec,0 α4,0 n−Bc Ec,0 C 1,0 ac1,0 = Ac Ec,0 α3,0 C (A.57a,b)

ac2,0 =

Ac Ec,0 α2,0 p−Bc Ec,0 α1,0 p 2

(A.57c)

and Mc,0 = Bc Ec,0 u0 − Ic Ec,0 v0 z2 = Bc Ec,0 α2,0 p + α3,0 C1,0 + α4,0 n z + C5,0 2 z2 2,0 − Ic Ec,0 α1,0 p + C1,0 z + C 2 = bc0,0 + bc1,0 z + bc2,0 z2

(A.58)

where: 5,0 −Ic Ec,0 C 2,0 ; bc0,0 = Bc Ec,0 C

1,0 +Bc Ec,0 α4,0 n−Ic Ec,0 C 1,0 bc1,0 = Bc Ec α3,0 C (A.59a,b)

bc2,0 =

Bc Ec,0 α2,0 p−Ic Ec,0 α1,0 p 2

(A.59c)

A.5.2 Age-adjusted effective modulus method (AEMM) The differential equations and boundary conditions to be used for the time analysis require the knowledge of the functions fcrN and fcrM in Eqs A.47 and A.48. Expressions for these terms to be used with the AEMM can be obtained substituting Eqs A.56 and A.58 into Eqs A.14: fcrN = Fe,0 Nc,0 = Fe,0 ac0,0 + ac1,0 z + ac2,0 z2 fcrM = Fe,0 Mc,0 = Fe,0 bc0,0 + bc1,0 z + bc2,0 z2

(A.60a) (A.60b)

and their ﬁrst and second derivatives, included in the system of differential equations, become: fcrN = Fe,0 ac1,0 + 2ac2,0 z ; fcrN = 2ac2,0 Fe,0 ;

fcrM = Fe,0 bc1,0 + 2bc2,0 z

fcrM = 2bc2,0 Fe,0

(A.61a,b) (A.61c,d)

Shrinkage effects are included using the same approach adopted for the ﬁnite element formulation in Section A4.1 where both fshN and fshM (related to shrinkage) are

414 Analytical formulations assumed to remain constant along the member length and when used with the AEMM are: fshN =

Ac

Ee,k Ac εsh,k and fshM = Ee,k εsh,k dA =

Ac

y Ee,k εsh,k dA = Ee,k Bc εsh,k (A.62a,b)

It is now possible to solve the differential equations (Eqs A.47) as a function of the axial displacement and deﬂection at time τk by substituting Eqs A.60 and A.62 into Eqs A.47: z3 z2 uk = α2,k p + β2,k + α3,k C1,k + α4,k n + β3,k + C5,k z + C6,k 6 2 z4 z3 z2 + C1,k + C2,k + C3,k z + C4,k vk = α1,k p + β1,k 24 6 2

(A.63a) (A.63b)

where the constants αi,k (i = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τk and the constants βi,k (i = 1 to 3) are given by: β1,k =

2RA bc2,0 Fe,0 − 2RB ac2,0 Fe,0 α0,k

β2,k =

RB 2ac2,0 Fe,0 β1,k − RA RA

and β3,k = −

(A.64a) ac1,0 Fe,0 RA

(A.64b,c)

The equivalent nodal loads required to account for member loads, creep and shrinkage are determined in the following worked example. A.5.2.1 Equivalent nodal actions at time τk Consider the ﬁxed-ended beam of the previous sections (shown in Fig. A.7) subjected to constant member loads n and p, as well as creep and shrinkage effects. The equivalent nodal loads required in the stiffness method to simulate member loads, creep and shrinkage effects are here determined separately using the general solution in Eqs A.63. From the boundary conditions for the ﬁxed ended beam (i.e. uL,k = uR,k = vL,k = vR,k = θL,k = θR,k = 0), the following expressions for the constants of integration are determined: C1,k = −

C5,k =

α1,k p + β1,k L; 2

C2,k =

α1,k p + β1,k 2 L ; 12

C3,k = 0;

C4,k = 0 (A.65a–d)

3α1,k α3,k − 2α2,k 2 α4,k α3,k L2 L2 L L p− n+ β1,k − β − β ; C6,k = 0. 12 2 4 6 2,k 2 3,k (A.65e,f)

Analytical formulations 415 and the support reactions are then obtained solving (Eqs A.48): RA uL,k −RB vL,k +fcrNL −fshNL +NL = 0;

RA uR,k −RB vR,k +fcrNR −fshNR −NR = 0;

+fcrML −fshML +SL = 0; RB uL,k −RI vL,k

RB uR,k −RI vR,k +fcrMR −fshMR −SR = 0;

+fcrML −fshML −ML = 0; RB uL,k −RI vL,k

RB uR,k −RI vR,k +fcrMR −fshMR +MR = 0.

The results have been summarized below for each loading condition considered separately. The three sets of reactions pF.m , pF.sh and pF.cr are the opposite of the equivalent nodal loads required in the stiffness method to handle these loading conditions: ⎤ ⎡ ⎤ ⎡ ⎡ ⎤ ⎡ ⎤ 0 NL.m Ee,k Ac εsh,k −L/2 ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎢ ⎢ α3,k ⎥ 0 ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ 2 ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L /12⎥ ⎢−Ee,k Bc εsh,k ⎥ ⎢Lα3,k /2⎥ pF.m = ⎢ ⎥=⎢ ⎥ ⎥ p+⎢ ⎥ n; pF.sh = ⎢ ⎥ ⎢ NR.m ⎥ ⎢ 0 ⎥ ⎢− ⎢ −L/2 ⎥ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ ⎢ Ee,k Ac εsh,k ⎥ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ ⎥ 0 ⎦ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ ⎣ ⎣ −α3,k ⎦ 2 L /12 MR.m Lα3,k /2 Ee,k Bc εsh,k ⎡

ac2,0 L2 ac1,0 L + + ac0,0 − Fe,0 3 2

(A.66a,b)

⎤

⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 ⎢ ⎥ ac1,0 + ac2,0 L L ⎢ ⎥ − L − b + b α − F e,0 c0,0 c2,0 3,k ⎢ ⎥ 2 6 ⎢ ⎥ pF.cr = ⎢ ⎥ 2 ⎢ ⎥ a L L a c2,0 c1,0 ⎢ ⎥ Fe,0 + + ac0,0 ⎢ ⎥ 3 2 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ − Fe,0 α3,k ac1,0 + Lα3,k ac2,0 − bc1,0 − bc2,0 L ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ 2 ac1,0 + ac2,0 L 5L ⎦ ⎣ −Fe,0 − α3,k L + bc0,0 + bc1,0 L + bc2,0 2 6

(A.66c)

A.5.2.2 Post-processing of the solution at time τk The expressions for uk and vk to be used in the post-processing are given in Eqs A.63. Considering that both creep and shrinkage have been included in the analysis using equivalent nodal actions it is necessary to solve the governing system of differential equations at time τk (Eqs A.47) using the nodal displacements at that time as boundary conditions. The relevant constants of integration (for Eqs A.63) can be obtained using Eqs A.48 as: 1,k = − α1,k p+β1,k L+ 6 θR,k +θL,k − 12 vR,k −vL,k ; C 2 3 2 L L

3,k = θR,k C (A.67a,b)

416 Analytical formulations α 2,k = 1,k p+β1,k L2 − 2 θR,k +2θL,k + 6 vR,k −vL,k ; C 2 12 L L 5,k = C

6,k = uL,k . 4,k = vL,k ; C C

3α1,k α3,k −2α2,k 2 α4,k α3,k L2 L2 L L p− n+ β1,k − β2,k − β3,k 12 2 4 6 2 6α3,k uR,k −uL,k 3α3,k − θR,k +θL,k − 2 vL,k −vR,k + L L L

(A.67c–e)

(A.67f)

Based on these, the expressions for uk and vk which deﬁne the strain diagram at τk can be written as: z2 1,k + α4,k n + β3,k z + C 5,k uk = α2,k p + β2,k + α3,k C 2 z2 2,k 1,k z + C +C vk = α1,k p + β1,k 2

(A.68a) (A.68b)

For completeness, the expressions for the internal actions resisted by the concrete at τk can be determined as follows: Ee,k uk − Bc Ee,k vk − Ac Ee,k εsh,k + Fe,0 Nc,0 Nc.k = Ac z2 1,k + α4,k n + β3,k z + C 5,k = Ac Ee,k α2,k p + β2,k + α3,k C 2 z2 1,k z + C 2,k − Bc Ee,k α1,k p + β1,k +C 2 − Ac Ee,k εsh,k + Fe,0 ac0,0 + ac1,0 z + ac2,0 z2 = ac0,k + ac1,k z + ac2,k z2

(A.69a)

Mc.k = Bc Ee,k uk − Ic Ee,k vk − Bc Ee,k εsh,k + Fe,0 Mc,0 z2 = Bc Ee,k α2,k p + β2,k + α3,k C1,k + α4,k n + β3,k z + C5,k 2 z2 − Ic Ee,k α1,k p + β1,k + C1,k z + C2,k 2 − Bc Ee,k εsh,k + Fe,0 bc0,0 + bc1,0 z + bc2,0 z2 = bc0,k + bc1,k z + bc2,k z2

(A.69b)

where: 5,k − Bc 2,k − Ac Ee,k C Ee,k C Ee,k εsh,k + Fe,0 ac0,0 ac0,k = Ac 1,k + α4,k n + β3,k − Bc 1,k + ac1,k = Ac Ee,k α3,k C Ee,k C Fe,0 ac1,0

(A.70a) (A.70b)

Analytical formulations 417 α p + β α p + β 2,k 2,k 1,k 1,k Ee,k Ee,k (A.70c) − Bc + Fe,0 ac2,0 ac2,k = Ac 2 2 5,k − Ic 2,k − Bc bc0,k = Bc Ee,k C Ee,k C Ee,k εsh,k + Fe,0 bc0,0

(A.70d)

1,k + α4,k n + β3,k − Ic 1,k + bc1,k = Bc Ee,k α3,k C Ee,k C Fe,0 bc1,0

(A.70e)

Ee,k bc2,k = Bc

α2,k p + β2,k α1,k p + β1,k − Ic Ee,k + Fe,0 bc2,0 2 2

(A.70f)

A.5.3 Step-by-step method (SSM) The time-dependent response of a beam segment calculated using the SSM is obtained by solving the system of differential (Eqs A.47) and corresponding boundary conditions (Eqs A.48) at time τk using the following expressions for fcrN,k and fcrM,k (Eqs A.15):

fcrN,k =

k−1 i=0

fcrM,k =

k−1 i=0

Ac

Fe,k,i σc,i dA =

k−1

(A.71a)

i=0

Ac

Fe,k,i Nc,i

yFe,k,i σc,i dA =

k−1

Fe,k,i Mc,i

(A.71b)

i=0

where the coefﬁcient Fe,k,i are deﬁned in Eq. 4.25, while the internal actions resisted by the concrete at times τi (Nc,i and Mc,i ) are given in Eqs A.39. It is assumed that the internal actions (i.e. Nc,n and Mc,n ) resisted by the concrete in previous time steps τn (with n = 0, . . . , i − 1) are known and available. Based on the fact that the format of the polynomials or functions describing the concrete internal actions do not vary with time, it is possible to derive the basic expressions for Nc,n and Mc,n from the results of the instantaneous analysis. This was already carried out when considering the AEMM leading to the use of parabolic expressions for both Nc,n and Mc,n (Eqs A.56 and A.58) assuming both member loads n and p to remain constant. These can be written for the generic time step τn required in Eqs A.39 as: Nc,n = ac0,n + ac1,n z + ac2,n z2

(A.72a)

Mc,n = bc0,n + bc1,n z + bc2,n z2

(A.72b)

where the coefﬁcients ac0,n and bc0,n are assumed to be known for n < i. The coefﬁcients describing the internal actions at time τi are obtained in the following by substituting ui and vi determined at time τi into Eqs A.39. For this purpose, the expressions for ui and vi are obtained by solving the system of differential equations of Eqs A.47 enforcing the kinematic boundary conditions consistent with the nodal displacements calculated from the stiffness method at time τi .

418 Analytical formulations The functions fcrN,i and fcrM,i are obtained substituting Nc,n and Mc,n into Eqs A.71:

fcrN,i =

i−1 n=0 Ac

Fe,i,n σc,n dA =

i−1

Fe,i,n Nc,n =

n=0

i−1

Fe,i,n ac0,n + ac1,n z + ac2,n z2

n=0

(A.73a) fcrM,i =

i−1 n=0 Ac

yFe,i,n σc,n dA =

i−1

Fe,i,n Mc,n =

n=0

i−1

Fe,i,n bc0,n + bc1,n z + bc2,n z2

n=0

(A.73b) and their ﬁrst and second derivatives become: fcrN,i =

i−1

Fe,i,n ac1,n + 2ac2,n z ;

fcrM,i =

n=0 fcrN,i

=

i−1

i−1

Fe,i,n bc1,n + 2bc2,n z

(A.74a)

n=0

2ac2,n Fe,i,n ;

n=0

fcrM,i

=

i−1

2bc2,n Fe,i,n

(A.74b)

n=0

Under the assumptions of constant shrinkage exhibited along the member length, the expressions for fshN,i and fshM,i are: fshN,i =

Ac

Ec,i εsh,i dA = Ec,i Ac εsh,i and fshM,i =

Ac

yEc,i εsh,i dA = Ec,i Bc εsh,i (A.75a,b)

Substituting Eqs A.73 to A.75 into Eqs A.47 the system of differential equations can be written at time τi as: RA ui − RB vi +

i−1

Fe,i,n ac1,n + 2ac2,n z + n = 0

(A.76a)

Fe,i,n bc1,n + 2bc2,n z + p = 0

(A.76b)

n=0

RB ui − RI vi +

i−1 n=0

This can be solved for ui and vi giving: z3 2 1,i + α4,i n + β3,i z + C 6,i 5,i z + C + α3,i C ui = α2,i p + β2,i 6 2 3 2 z4 1,i z + C 2,i z + C 3,i z + C 4,i +C vi = α1,i p + β1,i 24 6 2

(A.77a) (A.77b)

Analytical formulations 419 where the constants αj,i (j = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τi and the constants βj,i (j = 1 to 3) are given by: 2RA β1,i =

i−1 0

bc2,n Fe,i,n − 2RB

n=0

i−1 0

ac2,n Fe,i,n

n=0

(A.78a)

α0,i

RB β2,i = β1,i − RA

2

i−1 0

i−1 0

ac2,n Fe,i,n

n=0

RA

and β3,i = −

ac1,n Fe,i,n

n=0

(A.78b,c)

RA

The constants of integration required to deﬁne the displacements along the member lengths based on the solution at time τi (i.e. ui and vi ) are obtained by enforcing the boundary conditions at that time and are given by: 1,i = − α1,i p+β1,i L+ 6 θR,i +θL,i − 12 vR,i −vL,i ; C 3,i = θL,i C 2 3 2 L L 4,i = vL,i ; 2,i = α1,i p+β1,i L2 − 2 θR,i +2θL,i + 6 vR,i −vL,i ; C C 2 12 L L 2 2 5,i = 3α1,i α3,i −2α2,i L2 p− α4,i n+ α3,i L β1,i − L β2,i − L β3,i C 12 2 4 6 2 6α3,i uR,i −uL,i 3α3,i − 2 vL,i −vR,i + − vR,i +vL,i L L L

(A.79a,b) 6,i = uL,i C (A.79c–e)

(A.79f)

For the time instant τi the strain diagram can be deﬁned by substituting the constants of integration of Eqs A.79 into Eqs A.77 and differentiating: z2 5,i 1,i + α4,i n + β3,i z + C + α3,i C ui = α2,i p + β2,i 2 z2 2,i 1,i z + C +C vi = α1,i p + β1,i 2

(A.80a) (A.80b)

Substituting Eqs A.80 with the calculated constants of integrations (Eqs A.79) into Eqs A.39 gives: Nc.i = Ac Ec,i ui − Bc Ec,i vi − Ac Ec,i εsh,i +

i−1

Fe,i,n Nc,n

n=0

z2 1,i + α4,i n + β3,i z + C 5,i = Ac Ec,i α2,i p + β2,i + α3,i C 2 z2 − Bc Ec,i α1,i p + β1,i + C1,i z + C2,i 2

420 Analytical formulations − Ac Ec,i εsh,i +

i−1

Fe,i,n ac0,n + ac1,n z + ac2,n z2

n=0

= ac0,i + ac1,i z + ac2,i z2

(A.81)

where: 5,i − Bc Ec,i C 2,i − Ac Ec,i εsh,i + ac0,i = Ac Ec,i C

i−1

Fe,i,n ac0,n

(A.82a)

n=0 i−1 1,i + α4,i n + β3,i − Bc Ec,i C 1,i + ac1,i = Ac Ec,i α3,i C Fe,i,n ac1,n

(A.82b)

n=0

α2,i p + β2,i α1,i p + β1,i Fe,i,n ac2,n − Bc Ec,i + 2 2 i−1

ac2,i = Ac Ec,i

(A.82c)

n=0

Similarly, for Mc,i : Mc,i = Bc Ec,i ui − Ic Ec,i vi − Bc Ec,i εsh,i +

i−1

Fe,i,n Mc,n

n=0

z2 5,i 1,i + α4,i n + β3,i z + C = Bc Ec,i α2,i p + β2,i + α3,i C 2 z2 2,i 1,i z + C − Ic Ec,i α1,i p + β1,i +C 2 − Bc Ec,i εsh,i +

i−1

Fe,i,n bc0,n + bc1,n z + bc2,n z2

n=0

= bc0,i + bc1,i z + bc2,i z2

(A.83)

where: 5,i − Ic Ec,i C 2,i − Bc Ec,i εsh,i + bc0,i = Bc Ec,i C

i−1

Fe,i,n bc0,n

(A.84a)

n=0 i−1 1,i + α4,i n + β3,i − Ic Ec,i C 1,i + bc1,i = Bc Ec,i α3,i C Fe,i,n bc1,n

(A.84b)

n=0

α2,i p + β2,i α1,i p + β1,i − Ic Ec,i + Fe,i,n bc2,n 2 2 i−1

bc2,i = Bc Ec,i

(A.84c)

n=0

It is now possible to address the solution of the problem at time τk which will be used in the following example to determine the equivalent nodal actions to be used with

Analytical formulations 421 the SSM. This is now possible as the loading history of the concrete can be calculated and recorded for each previous time step τi (i < k) based on Eqs A.81 and A.83. Also, these can be used to deﬁne the expressions for fcrN.k and fcrM.k (Eqs A.14) required in the solution based on the creep effects due to stress increments at all previous time instants: fcrN,k =

k−1

Fe,k,i Nc,i =

i=0

fcrM,k =

k−1

Fe,k,i ac0,i + ac1,i z + ac2,i z2

(A.85a)

Fe,k,i bc0,i + bc1,i z + bc2,i z2

(A.85b)

i=0

k−1

Fe,k,i Mc,i =

i=0

k−1 i=0

with corresponding derivatives: fcrN,k =

k−1

Fe,k,i ac1,i + 2ac2,i z

and fcrM =

i=0

k−1

Fe,k,i bc1,i + 2bc2,i z

i=0

(A.86a,b) fcrN =

k−1

2ac2,i Fe,k,i

i=0

and fcrM =

k−1

2bc2,i Fe,k,i

(A.86c,d)

i=0

Using the notation adopted for the SSM, the shrinkage effects are: fshN,k =

Ac

Ec,k εsh,k dA = Ec,k Ac εsh,k and fshM,k =

Ac

yEc,k εsh,k dA = Ec,k Bc εsh,k (A.87a,b)

Substituting Eqs A.85 and A.87 into Eqs A.47 produces the governing system of differential equations: RA uk − RB vk +

k−1

Fe,k,i ac1,i + 2ac2,i z + n = 0

(A.88a)

Fe,k,i bc1,i + 2bc2,i z + p = 0

(A.88b)

i=0

RB uk − RI vk +

k−1 i=0

whose general solution can be expressed as: z3 z2 + α3,k C1,k + α4,k n + β3,k + C5,k z + C6,k uk = α2,k p + β2,k 6 2 z4 z3 z2 + C1,k + C2,k + C3,k z + C4,k vk = α1,k p + β1,k 24 6 2

(A.89a) (A.89b)

422 Analytical formulations where the constants αj,k (j = 0 to 4) are given in Eqs A.50 using the cross-sectional rigidities at time τk and the constants βj,i (j = 1 to 3) are given by:

2RA

k−1 0 i=0

β1,k =

k−1 0

bc2,i Fe,k,i − 2RB

i=0

ac2,i Fe,k,i

RB β2,k = β − RA 1,k

;

α0,k

2

k−1 0 i=0

ac2,i Fe,k,i RA (A.90a,b)

k−1 0

β3,k = −

i=0

ac1,i Fe,k,i (A.90c)

RA

A.5.3.1 Equivalent nodal actions at time τk Based on the ﬁxed-ended beam of the previous section (Fig. A.7), the expressions for the equivalent nodal loads required to account for member loads n and p, creep effects and shrinkage effects in the stiffness method are here determined using the SSM. The constants of integration to deﬁne the expressions for the axial displacement uk and deﬂection vk at time τk are identical to those obtained for the AEMM (and given in Eqs A.65) as the material properties are included in the coefﬁcients αj,k and βj,k . The end reactions at the ﬁxed supports are then obtained applying the static boundary conditions of Eqs A.48: + fcrNL,k − fshNL,k + NL = 0 RA uL,k − RB vL,k + fcrNR,k − fshNR,k − NR = 0 RA uR,k − RB vR,k + fcrML,k − fshML,k + SL = 0 RB uL,k − RI vL,k + fcrMR,k − fshMR,k − SR = 0 RB uR,k − RI vR,k + fcrML,k − fshML,k − ML = 0 RB uL,k − RI vL,k + fcrMR,k − fshMR,k + MR = 0 RB uR,k − RI vR,k

The vectors pF.m , pF.sh and pF.cr can be deﬁned as: ⎡

NL.m

⎤

⎡

0

⎤

⎡

−L/2

⎤

⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ α3,k ⎥ ⎢ SL.m ⎥ ⎢ −L/2 ⎥ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎢ ⎥ ⎢ML.m ⎥ ⎢−L2 /12⎥ ⎥=⎢ ⎥ p + ⎢Lα3,k /2⎥ n; pF.m = ⎢ ⎢ −L/2 ⎥ ⎢N ⎥ ⎢ 0 ⎥ ⎥ ⎢ ⎥ ⎢ R.m ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ ⎢ ⎣ −α3,k ⎦ ⎣ SR.m ⎦ ⎣ −L/2 ⎦ MR.m

L2 /12

Lα3,k /2

⎡

Ec,k Ac εsh,k

⎤

⎥ ⎢ ⎥ ⎢ 0 ⎥ ⎢ ⎢−Ec,k Bc εsh,k ⎥ ⎥ pF.sh = ⎢ ⎢−E A ε ⎥ (A.91a,b) ⎢ c,k c sh,k ⎥ ⎥ ⎢ ⎦ ⎣ 0 Ec,k Bc εsh,k

⎡

Analytical formulations 423 ⎤

k−1 0 ac2,i L2 ac1,i L ⎢ ⎥ F + + ac0,i − e,k,i ⎢ ⎥ 3 2 i=0 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ k−1 0 ⎢ ⎥ Fe,k,i α3,k ac1,i + Lα3,k ac2,i − bc1,i − bc2,i L ⎢ ⎥ ⎢ ⎥ i=0 ⎢ ⎥ ⎢ ⎥ 2 k−1 0 ac1,i + ac2,i L L ⎢ ⎥ − Fe,k,i − α3,k L − bc0,i + bc2,i ⎢ ⎥ ⎢ ⎥ 2 6 i=0 ⎥ pF.cr = ⎢ ⎢ ⎥ 2 k−1 ⎢ ⎥ 0 a L a L c2,i c1,i ⎢ ⎥ Fe,k,i + + ac0,i ⎢ ⎥ 3 2 i=0 ⎢ ⎥ ⎢ ⎥ ⎢ ⎥ k−1 0 ⎢ ⎥ − Fe,k,i α3,k ac1,i + Lα3,k ac2,i − bc1,i − bc2,i L ⎢ ⎥ ⎢ ⎥ i=0 ⎢ ⎥ ⎢ k−1 ⎥ 2 ac1,i + ac2,i L 5L ⎦ ⎣ 0 − Fe,k,i − α3,k L + bc0,i + bc1,i L + bc2,i 2 6 i=0

(A.91c)

As expected these loading vectors are very similar to those already calculated using the AEMM. For example, Eqs A.91 are identical to Eqs A.66 with the only difference relying on the way the instantaneous concrete modulus is determined with the AEMM and SSM. The equivalent nodal actions for use in the stiffness method are equal and opposite to pF.m , pF.cr and pF.sh . A.5.3.2 Post-processing of the solution at time τi In the case of the SSM the expressions for the axial displacement ui and deﬂection vi required for the post-processing of the solution at any time instant have already been derived in Eqs A.77. For a time τi , the constants of integration deﬁning ui and vi are obtained using Eqs A.79. The expressions for ui and vi deﬁning the strain diagram at τi are given in Eqs A.80. For completeness, the internal actions resisted by the concrete component can be determined using Eqs A.81 and A.83.

A.6 References 1. Bathe, K.-J. (2006). Finite Element Procedures. Prentice Hall, Pearson Education, New Jersey. 2. Reddy, J.N. (2004). An Introduction to the Finite Element Method. Third edition, McGraw-Hill, New York. 3. Gupta, A.K. and Ma, P.S. (1977). Error in eccentric beam formulation. International Journal for Numerical Methods in Engineering, 11, 1473–1483. 4. Crisﬁeld, M.A. (1991). The eccentricity issue in the design if plate and shell elements. Communications in applied Numerical Methods, 7, 47–56. 5. Ranzi, G. and Zona, A. (2007). A composite beam model including the shear deformability of the steel component. Engineering Structures, 29, 3026–3041.

Index

ACI 318-08 57–9, 62–4 Afﬁnity assumption 130 Age-adjusted: effective modulus for concrete 121; effective modulus method (AEMM) 119–28, 151–64, 244–56; modular ratio 122; transformed section 156 Aging 8, 22: effect of 8 Aging coefﬁcient 119, 122–5; equations for 123–4; graphs for 124 Aspect ratio, Ly /Lx 327 AS3600-2009 57–9, 60–2; models for creep and shrinkage 26–31 Axial deformation 49–51 Axial rigidity 141 Basic creep 5 Biaxial bending 224–59 Bridge decks, thermal gradients 342 Column 101, 335–40 Column strip 330 Composite cross-sections: concrete-concrete 189–222; steel-concrete 180–9 Compressive strength of concrete 24 Constitutive relationships for concrete 22, 100, 106, 122, 127, 130 Continuity stresses 341, 349 Continuous structures see Indeterminate structures Cover-controlled cracks 261 Cracking: cover-controlled cracks 261; crack control 75–96; direct tension cracking 91–6; simpliﬁed code approaches for ﬂexural cracking 76–83; tension chord model for ﬂexural cracking 83–91; cracked cross-sections: effective cracked sections 57; effect of creep 16; effect of shrinkage 20; short-term analysis 54–6, 265–79; time-dependent analysis: AEMM 279–88; step-by-step method 288–92; cracked members: deﬂection of 49–75, 301–4

crack spacing: direct tension 95; ﬂexural 83–7 crack width determination: direct tension 91–6; ﬂexural 76–91 crack width limits 44, 45; direct tension cracks 75, 91–6; ﬂexural cracks 75–91; primary cracks 53, 83, 260–1; recommended maximum design crack widths 45; secondary cracks 261; shrinkage cracks 91–6; tension stiffening 37, 52–4, 261–2 Creep coefﬁcient 8–9, 26–9 Creep function 8–9 Creep of concrete: basic creep 5; basic ﬂow 7; creep coefﬁcient 8–9, 26–9; creep function 8–9; creep problems 3; delayed elastic strain 7; drying creep 5; drying ﬂow 7; effect of: age at loading 8; relative humidity 6; size and shape of member 6; strength of concrete 6; stress level 6; temperature 6; effect on: axially loaded members 15; behaviour of structures 14–17; composite sections 187; fully-cracked reinforced concrete section 16; indeterminate prestressed members 320–2; moment–curvature relationship 264; slender columns 335–6; uncracked sections 16; ﬂow 7; inﬂuencing factors 5–6; integral-type creep law 13; irrecoverable creep 7; linear creep 6; mechanisms 5–6; non-linear creep 6; rapid initial ﬂow 7; recoverable creep 7; speciﬁc creep 9; tensile creep 14 Creep of prestressing steel 34–6 Crossing beam analogy 326 Cross-sectional analysis: cracked sections: short-term at time τ0 54–6, 265–79; time-dependent (AEMM) at τk 279–88; time-dependent (SSM) at τj 288–92; uncracked sections: short-term at time τ0 138–51, 189–92, 226–44; time-dependent (AEMM) at τk 119–28, 151–64, 192–4,

Index 425 244–56; time-dependent (SSM) at τj 105–19, 164–80, 200–3, 256–9 Cross-sectional rigidities: short-term at time τ0 140–2, 227–9, 269–70, 289; time-dependent (AEMM) at τk 154–5, 245–6, 280; time-dependent (SSM) at τj 167, 257, 291 Curvature: due to axial force and biaxial bending 224–5; due to axial force and uniaxial bending 137–8; due to creep 16; effect of non-prestressed steel on 297–301; integration of 50; due to shrinkage 20; due to temperature 341 Deﬂection: calculation from curvature at ends and at mid-span 49–52; calculation (recommended procedure) 69–75; at column mid-length 335–6; control using non-prestressed reinforcement 297–301; of cracked statically determinate beams 301–4; by double integration of curvature 50; in edge-supported slabs 326; in ﬂat slabs 330; incremental deﬂection 42–3; limits 41–4; long-term multiplication factor 58–9; problems 41–2; total deﬂection 42–3; of uncracked statically determinate beams 294–6 Delayed elasticity 7 Density of concrete 26 Depth to the neutral axis of a cracked section 54–5, 266–71 Designing for serviceability 38–44: crack width limits 44–5; deﬂection limits 41–4; design actions 39–41; design objectives and criteria 38–9; incremental deﬂection 42–3; total deﬂection 42–3; vibration control 44 Dischinger’s equation of state 130 Drying creep 5 Edge-supported two-way slab 326–30 Effective modular ratio 102 Effective modulus method (EMM) 100–5 Effective modulus of concrete 9, 100 Effective second moment of area (effective moment of inertia) 57 Eigenstresses: due to non-linear shrinkage 19; due to non-linear temperature 340 Elastic modulus of concrete 25–6 Elastic strain 2–3 Environmental loads 40 Equivalent nodal actions 411, 422 Euler-Bernoulli beam assumptions 261, 355, 391 Eurocode 2, 64–9, 77–9

Finite element analysis: for cracked members 387–90; formulation 396–406; for uncracked members 376–83 Flat slabs 330–5 Flexibility coefﬁcients 307 Flexibility matrix 307 Force method 306 Frame element 355 Indeterminate structures 305–24 Instantaneous concrete strain 2–3 Integral-type creep law 13 Irrecoverable creep 7 Kinematic model 392 Limit states design 39 Linear creep 6 Loads on structures: environmental loads 40; expected loads 40; load combinations for serviceability 40; speciﬁed (or characteristic) loads 40 Load versus deﬂection response 52–3 Long-term deﬂection multiplication factor 58 Loss of prestress 163, 301 Mechanisms of creep 5–6 Member loads 354 Middle strip 330 Modular ratio 54 Modular ratio theory 52, 54–6 Moment–curvature relationships 262–4 Moment redistribution 14, 20, 306, 320, 322 Non-linear creep 6 Non-linear strain distributions 19, 341 Non-linear temperature distributions 341–2 Non-prestressed steel 32–3 Parallel creep curve assumption 129 Post-processing solutions: instantaneous 412–13; time analysis 413–23 Post-tensioned beam 294 Prestressing steel 33–6 Pretensioned plank 323 Primary cracks 53, 83, 261 Primary structure 306 Principle of superposition 9–14, 105–19 Rate of creep method (RCM) 128–33 Redundant forces 305–16 Reinforcement see Steel reinforcement Relaxation of prestressing steel 34–6 Relaxation problems 3 Restrained shrinkage 20, 92

426

Index

Rigidities: short-term at time τ0 140–2, 227–9, 269–70, 289; time-dependent (AEMM) at τk 154–5, 245–6, 280; time-dependent (SSM) at τj 167, 257, 291 Secondary cracks 261 Secondary actions 320, 335, 341 Second moment of area: cracked section 53, 56; effective 53, 57; uncracked section 53 Serviceability limit states 39 Settlement of supports 316 Shrinkage of concrete: autogenous shrinkage 17; chemical shrinkage 17 drying shrinkage 17, 30; effect of: aggregate type, 18; relative humidity 18; size and shape of member 18; water–cement ratio 18; effect on: behaviour of structures 18–22; moment–curvature relationship 264; eigenstresses 19; endogenous shrinkage 17, 29–30; induced tension 20, 57; inﬂuencing factors 18; method for predicting 29–31; non-linear distribution 19; plastic shrinkage 17; prediction of 29–31; self-equilibrating stresses 19, 340–1; shrinkage-induced curvature 20; thermal shrinkage 17 Sign convention xiv–xix Slab stiffness factor 327 Slabs see Two-way slabs Slender columns 335–40; iterative analysis 336; primary and secondary moments 335 Slope 50 Solar radiation 341 Span-to-depth ratio 44–9 Speciﬁc creep 9 Statically determinate members 293–4 Statically indeterminate members 305–24; determination of redundants 306–8; effect of support settlement 316–17; effects of creep 320–2 Steel reinforcement 31–6; conventional or non-prestressed reinforcement 32–3; prestressing steel: creep coefﬁcient 35–6; relaxation 34–6; relaxation reduction due to concrete creep and shrinkage, 35–6; wire, strand and bar 33–6

Step-by-step method (SSM) 105–9, 256–9 Stiffness matrix 352, 410 Stiffness method 351–4 Strain components 2–3 Strain magnitudes 4–5 Superposition equation 11, 106–7 Support settlement 316–20 Temperature effects: coefﬁcients of thermal expansion 342; continuity stresses 349; cross-sectional analysis 341–4; eigenstresses 340; on magnitude of creep 6; non-linear distribution 341–2; redundant forces 347; self-equilibrating, 340 Tensile creep 14 Tensile strength of concrete 24–5 Tension chord model 83–91 Tension stiffening 37, 41, 52–4, 57, 70, 77, 84 Thermal effects see Temperature effects Time analyses: basic concepts 22; of cracked cross-sections 279–80, 290–1; ﬁnite element method 376–83, 387–90; of indeterminate members 305–8; stiffness method 361–3, 368; of uncracked cross-sections: axial loading 105–10, 114–17, 119–22, 127, 128–30; biaxial bending 244–7, 256–9; composite concrete-concrete sections 192–4; composite steel-concrete sections 180–2; reinforced and prestressed sections in uniaxial bending 151–7, 164–9 Time discretisation 105–6 Transformed section 143, 270 Trost-Bazant Method 119 Two-way slabs: deﬂection components 331; deﬂection models 325–6; deﬂection problems 324; edge-supported slabs 326–7; ﬁnite element models 325–6; ﬂat slabs 330–1; maximum span-to-depth ratio 46–7; wide beam method 330 Vibration control 44 Wide beam method 330

Thank you for interesting in our services. We are a non-profit group that run this website to share documents. We need your help to maintenance this website.